VALUES OF SOME PHYSICAL CONSTANTS Name
Symbol
Numerical value
Speed of light in vacuum Dielectric constant of vacuum...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

VALUES OF SOME PHYSICAL CONSTANTS Name

Symbol

Numerical value

Speed of light in vacuum Dielectric constant of vacuum Magnetic permeability of vacuum Planck constant

c 7 ε0 = 10 /(4πc2 ) μ0 = 4π·10−7 h = h/(2π) e eV a.u.m. m Mp Mn λ ¯ c = /(mc) a0 = 4πε0 2 /(me2 ) α =λ ¯ c /a0 2 R∞ = /(2ma02 )

2.9979·108 m/s 8.8542·10−12 F/m 1.2566·10−6 H/m 6.6262·10−34 J·s 1.0546·10−34 J·s 1.6022·10−19 C 1.6022·10−19 J 1.6605·10−27 kg 9.1096·10−31 kg 1.6726·10−27 kg 1.6749·10−27 kg 3.8616·10−13 m 5.2918·10−11 m 1/137.036 2.1799·10−18 J 13.605 eV 9.2741·10−24 J/T 5.0508·10−27 J/T 1.3806·10−23 J/K 6.0221·1023 mole−1 8.3145 J·mole−1 ·K−1 1.1605·104 K 2.4180·1014 Hz 1.2398·10−6 m

Elementary charge Electron-volt Atomic unit of mass Electron mass at rest Proton mass at rest Neutron mass at rest Compton wavelength of electrons Bohr radius Fine structure constant Rydberg constant Bohr magneton Nuclear magneton Boltzmann constant Avogadro number Universal gas constant Temperature for kB T = 1 eV Frequency for hν = 1 eV Wavelength for hc/λ = 1 eV

μB = e/(2m) μn = e/(2Mp ) kB NA R = kB N A

CONVENTIONAL UNIT CELLS OF THE 14 BRAVAIS LATTICES

ENCYCLOPEDIC DICTIONARY OF CONDENSED MATTER PHYSICS

This Page Intentionally Left Blank

ENCYCLOPEDIC DICTIONARY OF CONDENSED MATTER PHYSICS

VOLUME 1 A–M EDITED BY

CHARLES P. POOLE JR. Department of Physics and Astronomy University of South Carolina Columbia, SC, USA

2004 Amsterdam – Boston – Heidelberg – London – New York – Oxford Paris – San Diego – San Francisco – Singapore – Sydney – Tokyo

ELSEVIER B.V. Sara Burgerhartstraat 25 P.O. Box 211, 1000 AE Amsterdam The Netherlands

ELSEVIER Inc. 525 B Street, Suite 1900 San Diego, CA 92101-4495 USA

ELSEVIER Ltd The Boulevard, Langford Lane Kidlington, Oxford OX5 UK

ELSEVIER Ltd 84 Theobalds Road 1GB London WC1X 8RR UK

© 2004 Elsevier Inc. All rights reserved. This work is protected under copyright by Elsevier Inc., and the following terms and conditions apply to its use: Photocopying Single photocopies of single chapters may be made for personal use as allowed by national copyright laws. Permission of the Publisher and payment of a fee is required for all other photocopying, including multiple or systematic copying, copying for advertising or promotional purposes, resale, and all forms of document delivery. Special rates are available for educational institutions that wish to make photocopies for non-proﬁt educational classroom use. Permissions may be sought directly from Elsevier’s Rights Department in Oxford, UK: phone (+44) 1865 843830, fax (+44) 1865 853333, e-mail: [email protected]. Requests may also be completed on-line via the Elsevier homepage (http://www.elsevier.com/locate/permissions). In the USA, users may clear permissions and make payments through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA; phone: (+1) (978) 7508400, fax: (+1) (978) 7504744, and in the UK through the Copyright Licensing Agency Rapid Clearance Service (CLARCS), 90 Tottenham Court Road, London W1P 0LP, UK; phone: (+44) 20 7631 5555; fax: (+44) 20 7631 5500. Other countries may have a local reprographic rights agency for payments. Derivative Works Tables of contents may be reproduced for internal circulation, but permission of the Publisher is required for external resale or distribution of such material. Permission of the Publisher is required for all other derivative works, including compilations and translations. Electronic Storage or Usage Permission of the Publisher is required to store or use electronically any material contained in this work, including any chapter or part of a chapter. Except as outlined above, no part of this work may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, without prior written permission of the Publisher. Address permissions requests to: Elsevier’s Rights Department, at the fax and e-mail addresses noted above. Notice No responsibility is assumed by the Publisher for any injury and/or damage to persons or property as a matter of products liability, negligence or otherwise, or from any use or operation of any methods, products, instructions or ideas contained in the material herein. Because of rapid advances in the medical sciences, in particular, independent veriﬁcation of diagnoses and drug dosages should be made. This is a translation from Russian. First edition 2004 Library of Congress Cataloging in Publication Data: A catalog record is available from the Library of Congress. British Library Cataloguing in Publication Data: A catalogue record is available from the British Library. ISBN 0-12-088398-8 volume 1 ISBN 0-12-088399-6 volume 2 ISBN 0-12-561465-9 set ∞ The paper used in this publication meets the requirements of ANSI/NISO Z39.48-1992 (Permanence of Paper).

Printed in The United Kingdom.

EDITOR’S PREFACE TO THE ENGLISH EDITION At the present time Condensed Matter Physics is the largest of the main subdivisions of physics. For several years the Encyclopedic Dictionary of Solid State Physics has been one of the principal reference works in this area, but unfortunately until now it was only available in the Russian language. Its appearance in English is indeed long overdue. It has been a great pleasure for me to undertake the task of editing the English language edition. This two-volume work contains a great deal of material ordinarily not found in the solid state texts that are most often consulted for reference purposes, such as accounts of acoustical holography, bistability, Kosterlitz–Thouless transition, and self-similarity. It provides information on materials rarely discussed in these standard texts, such as austenite, ferroﬂuids, intercalated compounds, laser materials, Laves phases, nematic liquid crystals, etc. Properties of many quasi-particles are presented; for example, those of crowdions, dopplerons, magnons, solitons, vacancions, and weavons. The volumes are fully cross-referenced for tracking down all aspects of a topic, and in this respect we have emulated the excellent cross-referencing systematics of the Russian original. Long lists of alternate titles for looking up subjects can considerably shorten the time needed to ﬁnd specialized information. I wish to thank the members of the Review Panel of the English Language Edition who read over the initial draft of the translation, offered many suggestions and comments for improving the translation, and also provided valuable advice for reﬁning and updating the contents of the articles: Victor Bar’yakhtar, Alexei A. Maradudin, Michael McHenry, Laszlo Mihaly, Sergey K. Tolpygo and Sean Washburn. Thanks are also due to Horacio A. Farach, Vladimir Gudkov, Paul G. Huray, Edwin R. Jones, Grigory Simin, Tangali S. Sudarshin, and especially to Ruslan Prozorov, for their assistance with the editing. The translators did an excellent job of rendering the original Russian text into English, and the desk editor Rimantas Šadžius v

vi

did an outstanding job of checking all the many cross references and the consistency of the notation. The Academic Press Dictionary of Science and Technology has been an invaluable source of information for clarifying various issues during the editing. I wish to thank my wife for her patience with me during the long hours expended in the editing process. The page proofs of this work arrived at my home on the octave day of our 50th wedding anniversary, which we celebrated on October 17, 2003, with our ﬁve children and ﬁfteen grandchildren. Charles P. Poole Jr.

FOREWORD An Encyclopedic Dictionary of Condensed Matter Physics can serve a diverse set of audiences. Professional researchers and university and college teachers interested in learning quickly about a topic in condensed matter physics outside their immediate expertise can obtain the information they seek from such a source. Doctoral students embarking on research in condensed matter physics or materials science can ﬁnd it helpful in providing explanations of concepts and descriptions of methods encountered in reading the literature dealing with their research subject and with related subjects. Undergraduate students with no previous background in condensed matter physics will ﬁnd it a particularly valuable complement to their textbooks as they take their ﬁrst courses in the ﬁeld. Educated laypersons can turn to such an encyclopedia for help in understanding articles published in popular scientiﬁc journals. Until the publication of the Russian edition of the Encyclopedic Dictionary of Solid State Physics, with Professor Viktor G. Bar’yakhtar as its General Editor, no such resource was available to the scientiﬁc community. Its more than 4300 entries were written by more than 700 contributors, specialists in their branches of condensed matter physics, many of whom were well known to an international audience. The task of making this encyclopedia accessible to non-Russian readers was undertaken by Academic Press, with Professor Charles P. Poole Jr. in the role of the General Editor for the English translation. Both the publisher and editor deserve the gratitude of the condensed matter community for bringing this project to fruition. All involved in its production hope that that community will ﬁnd it as useful as its creators intended it to be.

Irvine, California October 29, 2003

Alexei A. Maradudin

vii

This Page Intentionally Left Blank

FOREWORD OF THE EDITORIAL BOARD OF THE ORIGINAL RUSSIAN EDITION This publication is an attempt at a systematized presentation of modern knowledge within all areas of solid state physics from the most fundamental ideas to applied questions. There has been no similar encyclopedic compilation of solid state physics available in the world until now. The Dictionary contains more than 4000 articles. Among them there are relatively long articles devoted to the basic concepts and phenomena of solid state physics, moderate-length articles on particular problems and physical concepts, and, ﬁnally, brief deﬁnitions of terms used in the literature. Considerable attention is paid to technical applications of solid state physics. Brief historical information is given in many articles such as the names of authors and the dates of discoveries. In a number of cases the history of the question is covered in the article. Together with the description of classical topics, special attention is paid to those new ideas that arose only recently in solid state physics and, therefore, often still do not have commonly accepted deﬁnitions. Many articles are provided with illustrations which supplement the text material to help the reader to acquire more complete and more visual information. More than 500 scientists participated in the preparation and the writing of the articles of the Dictionary; these articles were written by specialists working in the particular ﬁelds that they cover. The goal of the publication is to provide needed reference material to a wide audience of readers, which will help them to understand the basic principles of solid state physics. Therefore, the authors endeavored to probe deeply into some salient details of the subject, while preserving a broad perspective throughout the text of the article. The content of articles is interconnected by a system of cross-references. The appended Subject Index will help the reader to orient himself easily in the scope of the various articles. To our deep sorrow, during the period of preparation of the manuscript of this Dictionary, several outstanding scientiﬁc members of the Editorial Board Valentin L’vovich Vinetskii, Yakov Evseevich Geguzin, Emanuil Aizikovich Kaner, Boris Ivanovich Nikolin, Kirill Borisovich Tolpygo, Leonid Nikandrovich Larikov and Alexander Bronislavovich Roitsyn have passed from among us. The recently expired wellknown scientist and prominent publishing specialist Aleksandr Aleksandrovich Gusev, who shared with us his vast knowledge and encyclopedic expertise, provided invaluable aid in the publication of the dictionary. Victor G. Bar’yakhtar, Editor-in-Chief Ernest A. Pashitskii, Vice-Editor-in-Chief Elena G. Galkina, Secretary We started as the team (EDITORIAL BOARD OF THE ORIGINAL RUSSIAN EDITION): V.G. Bar’yakhtar, Editor-in-Cief V.L. Vinetskii, Vice-Editor-in-Chief E.A. Pashitskii, Vice-Editor-in-Chief E.G. Galkina, Secretary

A.S. Bakai Ya.E. Geguzin M.D. Glinchuk Yu.V. Gulyaev ix

B.A. Ivanov M.I. Kaganov E.A. Kaner A.P. Korolyuk

x

A.M. Kosevich L.N. Larikov V.G. Manzhelii

FOREWORD OF THE EDITORIAL BOARD OF THE ORIGINAL RUSSIAN EDITION

B.I. Nikolin A.B. Roitsyn

K.B. Tolpygo M.Ya. Valakh

SCIENTIFIC CONSULTANTS OF THE ORIGINAL RUSSIAN EDITION:

E.M. Baskin E.D. Belokolos L.G. Bugaenko B.M. Bulakh A.V. Chaplik I.M. Dmitrenko V.N. Dobrovol’skii M.I. Dykman B.N. Filippov V.A. Finkel’

V.L. Ginzburg A.V. Golik S.A. Gredeskul V.N. Grigor’yev A.A. Gusev M.A. Ivanov Yu.S. Kaganovskii A.E. Kiv Yu.V. Kornyushin E.N. Korol’

I.O. Kulik O.D. Lavrentovich N.M. Makarov G.D. Mansfel’d Yu.V. Mil’man V.M. Nadutov V.D. Natsyk M.E. Osinovskii L.S. Palatnik

S.S. Rozhkov S.M. Ryabchenko P.V. Ryabko A.V. Sachenko K.K. Shvarts A.A. Slutskin A.I. Sokolov V.A. Tatarenko A.F. Zhuravlev

LIST OF CONTRIBUTORS F.Kh. Abdullaev A.A. Adamovskii S.S. Afonskii I.A. Akhiezer A.F. Akkerman A.B. Aleinikov V.P. Alekhin A.S. Aleksandrov L.N. Aleksandrov B.L. Al’tshuler E.D. Aluker S.P. Anokhov L.I. Antonov K.P. Aref’ev I.E. Aronov M. Ashe Yu.E. Avotin’sh V.G. Babaev Yu.Z. Babaskin S.G. Babich Yu.I. Babii A.S. Bakai Yu.V. Baldokhin O.M. Barabash S.D. Baranovskii Z.V. Bartoshinskii V.G. Bar’yakhtar V.G. Baryshevskii E.M. Baskin F.G. Bass A.N. Bekrenev I.P. Beletskii Ya.A. Beletskii S.I. Beloborod’ko E.D. Belokolos V.F. Belostotskii A.V. Belotskii M.V. Belous

N.P. Belousov K.P. Belov D.P. Belozerov A.I. Belyaeva S.S. Berdonosov B.I. Beresnev L.I. Berezhinskii V.I. Bernadskii I.B. Bersuker V.N. Berzhanskii P.A. Bezirganyan V.F. Bibik I.V. Blonskii E.N. Bogachek A.N. Bogdanov Yu.A. Bogod S.A. Boiko V.S. Boiko S.I. Bondarenko V.N. Bondarev A.S. Borovik-Romanov A.A. Borshch Yu.S. Boyarskaya A.M. Bratkovskii O.M. Braun S.L. Bravina M.S. Bresler A.B. Brik M.S. Brodin V.A. Brodovoi L.T. Bugaenko V.N. Bugaev M. Buikov L.L. Buishvili E.I. Bukhshtab L.N. Bulaevskii B.M. Bulakh A.A. Bulgakov

S.I. Bulychev A.I. Buzdin A.I. Bykhovskii A.M. Bykov Yu.A. Bykovskii G.E. Chaika A.A. Chel’nyi S.P. Chenakin V.T. Cherepin N.F. Chernenko Yu.P. Chernenkov A.A. Chernov S.I. Chugunova B.A. Chuikov K.V. Chuistov A.A. Chumak V.E. Danil’chenko V.D. Danilov L.I. Datsenko A.B. Davydov A.S. Davydov S.A. Dembovskii V.L. Demikhovskii S.A. Demin E.M. Dianov V.V. Didyk I.M. Dmitrenko N.L. Dmitruk V.N. Dneprenko V.S. Dneprovskii V.N. Dobrovol’skii R.D. Dokhner I.F. Dolmanova F.E. Dolzhenkov V.F. Dorfman S.N. Dorogovtsev N.V. Dubovitskaya E.F. Dudnik xi

V.A. Durov V.V. Dyakin M.I. Dykman A.I. Eﬁmov A.L. Efros Yu.A. Ekmanis M.A. Elango V.M. Elinson P.G. Eliseev V.A. Elyukhin Yu.P. Emets V.V. Emtsev V.Z. Enol’skii I.R. Entin I.R. Entinzon E.M. Epshtein A.I. Erenburg A.S. Ermolenko E.D. Ershov A.M. Evstigneev M.I. Faingol’d V.M. Fal’chenko V.L. Fal’ko B.Ya. Farber M.P. Fateev I.M. Fedorchenko O.P. Fedorov A.G. Fedorus Ya.A. Fedotov I.V. Fekeshgazi A.V. Filatov B.N. Filippov V.A. Finkel’ V.M. Finkel’ A.Ya. Fishman N.Ya. Fogel’ E.L. Frankevich L.I. Freiman

xii

V.M. Fridkin I.Ya. Fugol’ B.I. Fuks A.M. Gabovich S.P. Gabuda A.Yu. Gaevskii Yu.A. Gaidukov V.P. Galaiko R.V. Galiulin Yu.M. Gal’perin M.Ya. Gamarnik G.D. Gamulya E.M. Ganapol’skii V.G. Gavrilyuk Ya.E. Geguzin B.L. Gel’mont D.S. Gertsriken I.A. Gilinskii I.A. Gindin S.L. Ginzburg E.I. Givargizov E.I. Gladyshevskii A.A. Glazer L.I. Glazman A.I. Glazov M.D. Glinchuk E.Ya. Glushko V.M. Gokhfel’d V.L. Gokhman V.A. GolenishchevKutuzov A.V. Golik M.F. Golovko T.V. Golub D.A. Gorbunov L.Yu. Gorelik Yu.I. Gorobets V.I. Gorshkov V.V. Gorskii V.G. Grachev S.A. Gredeskul V.P. Gribkovskii P.P. Grigaitis V.N. Grigor’ev O.N. Grigor’ev Yu.M. Grin’ V.V. Gromov V.V. Gudkov A.V. Gulbis

LIST OF CONTRIBUTORS

A.P. Gulyaev Yu.V. Gulyaev M.E. Gurevich Yu.G. Gurevich K.P. Gurov R.N. Gurzhi M.B. Guseva A.N. Guz’ V.M. Gvozdikov A.I. Ignatenko V.V. Il’chenko E.M. Iolin I.P. Ipatova S.S. Ishchenko Z.A. Iskanderova V. Iskra V.G. Ivanchenko P.G. Ivanitskii A.L. Ivanov B.A. Ivanov M.A. Ivanov N.R. Ivanov G.F. Ivanovskii P.F. Ivanovskii V.G. Ivantsov R.K. Ivashchenko O.M. Ivasishin Yu.A. Izyumov G.A. Kachurin A.N. Kadashchuk A.M. Kadigrobov M.I. Kaganov E.B. Kaganovich Yu.M. Kaganovskii N.P. Kalashnikov P.A. Kalugin G.G. Kaminskii E.A. Kaner L.N. Kantorovich A.S. Kapcherin A.A. Kaplyanskii A.L. Kartuzhanskii A.L. Kasatkin V.N. Kashcheev N.I. Kashirina G.A. Katrich B.V. Khaenko I.B. Khaibullin V.A. Kharchenko

E.I. Khar’kov S.S. Khil’kevich A.I. Khizhnyak G.E. Khodenkov A.R. Khokhlov G.A. Kholodar’ V.A. Khvostov K.I. Kikoin S.S. Kil’chitskaya O.V. Kirichenko A.P. Kirilyuk P.S. Kislyi A.E. Kiv Ya.G. Klyava V.M. Knyazheva E.S. Koba L.S. Kogan V.V. Kokorin Yu.A. Kolbanovskii G.Ya. Kolbasov A.G. Kol’chinskii V.L. Kolesnichenko V.V. Kolomiets V.I. Kolomytsev E.V. Kolontsova V.G. Kon A.A. Konchits S.N. Kondrat’ev M.Ya. Kondrat’ko V.A. Kononenko V.I. Konovalov A.I. Kopeliovich V.A. Koptsyk T.N. Kornilova Yu.V. Kornyushin E.N. Korol’ N.S. Kosenko A.M. Kosevich O.G. Koshelev A.S. Kosmodamianskii E.A. Kotomin N.Ya. Kotsarenko Yu.N. Koval’ V.V. Koval’chuk A.S. Kovalev O.V. Kovalev M.Yu. Kovalevskii Yu.Z. Kovdrya I.I. Kovenskii

V.I. Kovpak V.I. Kovtun A.V. Kozlov N.N. Krainik V.V. Krasil’nikov A.Ya. Krasovskii L.S. Kremenchugskii V.P. Krivitskii M.A. Krivoglaz V.N. Krivoruchko A.A. Krokhin S.P. Kruglov I.V. Krylova A.Yu. Kudzin L.S. Kukushkin I.O. Kulik V.A. Kuprievich A.I. Kurbakov A.V. Kurdyumov V.G. Kurdyumov G.G. Kurdyumova M.V. Kurik M.I. Kurkin N.P. Kushnareva V.A. Kuz’menko R.N. Kuz’min V.N. Kuzovkov A.I. Landau V.F. Lapchinskii L.N. Larikov F.F. Lavrent’ev O.D. Lavrentovich B.G. Lazarev L.S. Lazareva Ya.S. Lebedev B.I. Lev A.P. Levanyuk A.A. Levin I.B. Levinson V.A. Likhachev M.P. Lisitsa V.M. Lisitsyn V.A. Lisovenko F.V. Lisovskii P.G. Litovchenko V.G. Litovchenko V.S. Litvinov V.A. Lobodyuk V.M. Loktev V.F. Los’

LIST OF CONTRIBUTORS

D.V. Lotsko V.P. Lukomskii G.A. Luk’yanov V.A. L’vov S.N. Lyakhimets V.G. Lyapin B.Ya. Lyubov I.F. Lyuksyutov R.G. Maev V.M. Maevskii L.L. Makarov N.M. Makarov V.I. Makarov D.N. Makovetskii L.A. Maksimov V.V. Malashenko B.Z. Malkin G.D. Mansfel’d V.G. Manzhelii V.G. Marinin S.V. Marisova V.Ya. Markiv Yu.V. Martynenko T.Ya. Marusii S.V. Mashkevich V.S. Mashkevich T.V. Mashovets V.V. Maslov O.I. Matkovskii Z.A. Matysina V.F. Mazanko I.I. Mazin E.A. Mazur B.V. Mchedlishvili M.V. Medvedev V.K. Medvedev A.I. Mel’ker G.A. Melkov V.S. Mel’nikov F.F. Mende Yu.Ya. Meshkov G.A. Mesyats V.P. Mikhal’chenko V.S. Mikhalenkov V.V. Milenin V.K. Milinchuk Yu.V. Mil’man M.G. Mil’vidskii V.N. Minakov

xiii

E.V. Minenko D.N. Mirlin I.A. Misurkin V.Ya. Mitrofanov N.V. Morozovskii V.V. Moshchalkov N.P. Moskalenko S.A. Moskalenko V.N. Murzin V.P. Naberezhnykh T.A. Nachal’naya V.M. Nadutov E.L. Nagaev V.E. Naish N.G. Nakhodkin V.D. Natsyk A.G. Naumovets O.K. Nazarenko E.I. Neimark I.M. Neklyudov I.Yu. Nemish V.V. Nemoshkalenko S.A. Nepiiko V.A. Nevostruev S.A. Nikitov M.Yu. Nikolaev B.I. Nikolin A.B. Nikol’skii G.K. Ninidze A.I. Nosar’ N.N. Novikov N.V. Novikov V. Novozhilov S.G. Odulov V.I. Okulov E.F. Oleinik N.V. Olechnovich S.I. Olikhovskii B.Z. Ol’shanetskii A.N. Omel’yanchuk A.N. Orlov S.P. Oshkaderov M.E. Osinovskii S.S. Ostapenko E.L. Ostrovskaya D.E. Ovsienko R.P. Ozerov G.A. Pacharenko P.P. Pal’-Val’

S.V. Panyukov I.I. Papirov E.S. Parilis A.M. Parshin E.A. Pashitskii L.A. Pastur R.E. Pasynkov E.P. Pechkovskii G.P. Peka V.I. Peresada S.P. Permogorov V.G. Peschanskii I.S. Petrenko E.G. Petrov V.A. Petrov Yu.N. Petrov G.A. Petrunin V.Yu. Petukhov A.S. Pikovskii G.E. Pikus A.N. Pilyankevich V.I. Pipa F.V. Pirogov G.S. Pisarenko E.A. Pisarev L.P. Pitaevskii A.B. Plachenov B.T. Plachenov Yu.N. Podrezov A.E. Pogorelov V.Z. Polinger Yu.N. Polivanov V.V. Polotnyuk S.S. Pop Yu.M. Poplavko L.E. Popov V.E. Pozhar L.I. Pranyavichus A.I. Prikhna V.E. Primachenko V.G. Prokhorov G.I. Prokopenko P.P. Pugachevich V.V. Pustovalov V.I. Pustovoit A.P. Rachek V.A. Rafalovskii V.V. Rakitin E.I. Rau

B.S. Razbirin A.R. Regel’ V.R. Regel’ V.Yu. Reshetnyak Yu.Ya. Reutov I.S. Rez I.M. Reznik Yu.A. Reznikov D.R. Rizdvyanetskii A.B. Roitsyn O.V. Romankevich A.E. Romanov A.S. Rozhavskii S.S. Rozhkov V.V. Rozhkov E.Ya. Rudavskii A.V. Rudnev I.N. Rundkvist S.M. Ryabchenko P.V. Ryabkov K.P. Ryaboshapka V. Rybalka A.I. Ryskin V.I. Ryzhkov A.M. Sabadash V.A. Sablikov A.V. Sachenko M.V. Sadovskii O.G. Sarbei V.M. Schastlivtsev Yu.V. Sedletskii S.I. Selitser A.V. Semenov Yu.G. Semenov A.I. Senkevich T.N. Serditova T.N. Sergeeva S.E. Shafranyuk S.I. Shakhovtsova A.M. Shalaev B.N. Shalaev B.D. Shanina B.Ya. Shapiro I.G. Shaposhnikov O.D. Shashkov V.G. Shavrov D.I. Sheka V.I. Sheka R.I. Shekhter V.A. Shenderovskii

xiv

S.I. Shevchenko A.Ya. Shik V.B. Shikin Yu.M. Shirshov S.V. Shiyanovskii G.N. Shkerdin O.A. Shmatko A.S. Shpigel’ T.D. Shtepa E.I. Shtyrkov Yu.N. Shunin A.K. Shurin K.K. Shvarts E.A. Silin’sh A.F. Sirenko A.I. Sirko A.A. Sitnikova F.F. Sizov E.V. Skokan V.V. Skorokhod V.V. Sleptsov A.A. Slutskin A.A. Smirnov L.S. Smirnov G.A. Smolenskii O.V. Snitko V.I. Sobolev A.I. Sokolov I.M. Sokolov A.S. Sonin E.B. Sonin A. Sorokin M.S. Soskin A.L. Sozinov V.B. Spivakovskii I.E. Startseva A.N. Starukhin E.P. Stefanovskii M.F. Stel’makh I.A. Stepanov I.A. Stoyanov

LIST OF CONTRIBUTORS

M.I. Strashnikova V.I. Strikha V.I. Sugakov A.P. Sukhorukov S.V. Svechnikov V.M. Svistunov I.I. Sych A.K. Tagantsev G.A. Takzei A.P. Tankeev V.V. Tarakanov V.V. Tarasenko G.G. Tarasov Yu.V. Tarasov I.A. Tarkovskaya V.A. Tatarchenko V.A. Tatarenko I.I. Taubkin V.A. Telezhkin Yu.S. Tikhodeev L.V. Tikhonov E.A. Tikhonova B.L. Timan S.F. Timashev B.B. Timofeev V.B. Timofeev Yu.A. Tkhorik K.B. Tolpygo S.K. Tolpygo P.M. Tomchuk V.I. Tovstenko V.I. Treﬁlov O.A. Troitskii V.A. Trunov V.A. Tsekhomskii B.E. Tsekvava R. Tsenker B.S. Tsukerblat V.M. Tsukernik L.T. Tsymbal N.V. Tsypin

L.I. Tuchinskii A. Tukharinov E.A. Turov Yu.D. Tyapkin V.M. Tyshkevich V.A. Tyul’nin K.M. Tyutin A.A. Urusovskaya A.I. Ustinov B.K. Vainshtein S.B. Vakhrushev M.Ya. Valakh V.I. Val’d-Perlov A.A. Varlamov I.A. Vasil’ev L.I. Vasil’ev M.A. Vasil’ev F.T. Vas’ko A.V. Vedyaev B.G. Vekhter O.G. Vikhlii V.L. Vinetskii E.A. Vinogradov B.B. Vinokur V.M. Vinokurov Yu.P. Virchenko A.S. Vishnevskii I.M. Vitebskii N.A. Vitovskii V.I. Vladimirov V.V. Vladimirov N.A. Vlasenko A.D. Vlasov K.B. Vlasov O.G. Vlokh E.D. Vol A.F. Volkov P.Yu. Volosevich V.A. Voloshin V.D. Volosov S.V. Vonsovskii

D.L. Vorob’ev S.A. Vorob’ev Yu.V. Vorob’ev A.M. Voskoboinikov B.E. Vugmeister D.A. Yablonskii Yu.N. Yagodzinskii L.N. Yagupol’skaya Yu.I. Yakimenko B.I. Yakobson M.V. Yakunin V.A. Yampol’skii I.K. Yanson A.M. Yaremko A.A. Yatsenko A.F. Yatsenko I.A. Yurchenko Yu.F. Yurchenko P.A. Zabolotnyi V.A. Zagrebnov Yu.R. Zakis E.Ya. Zandberg I.M. Zaritskii E.V. Zarochentsev I.K. Zasimchuk E.E. Zasimchuk S.S. Zatulovskii E.A. Zavadskii P.Yu. Zavalii Yu.S. Zharkikh I.S. Zheludev G.N. Zhizhin A.F. Zhuravlev S.N. Zhurkov O.S. Zinets D.N. Zubarev M.D. Zviadadze L.O. Zvorykin B.B. Zvyagin I.P. Zvyagin

INTRODUCTION 1

We introduce to the reader the Encyclopedic Dictionary of Solid State Physics . This Dictionary was planned several years ago, and the aim of its compilers was not only to provide a wide audience of readers with comprehensive and detailed information about different processes, phenomena, and effects in the solid state, but also to enlarge our understanding of the modern terminology in which this information is presented. The latter was very important for the compilers, since they were united by the idea that the achievements of solid state physics during recent decades were due not only to the fantastic development of experimental techniques and the level of experimental skill, but were also due to the creation of a uniﬁed system of concepts and terms adequately reﬂecting the observed regularities and the depth of understanding of the physical processes taking place in solids. The balanced rhythm of the modern language of solid state physics is determined by the theory of symmetry. It governs all theoretical constructions and the coefﬁcients of the equations describing equilibrium and near-equilibrium states of a solid. The dynamic theory of a crystal lattice in the harmonic approximation, which is based on the discrete symmetry of ordered atomic arrangement in a crystal, is a classical example how symmetry considerations are utilized. Another “hidden” symmetry is used, e.g., to describe a number of properties of magnetic, ferroelectric, and superconducting materials. A particular kind of symmetry based on the regularities in diverse phase transitions is apparent in modern scaling theory. The reader will ﬁnd applications of the theory of symmetry in many of the articles. The majority of the phenomena of recent interest in solids were associated with low-level excited states of a substance. It appeared that while atoms or molecules are structural elements of a crystal lattice (and, generally, of any condensed state of a substance), certain collective excitations are the elements of every type of motion (elements of dynamics) in a solid. In view of the macroscopic homogeneity of the unbounded model of a solid, or the periodicity of an unbounded crystal lattice, such collective motions must take the form of plane waves, with a dispersion law that satisﬁes strict symmetry requirements. The quantization of elementary excitations leads to the image of a “corpuscle”, or a quasi-particle. The concept of a quasi-particle and the idea of almost ideal quantum gases composed of various quasi-particles, enrich the language of solid state physics and allow one, within a uniﬁed system of terms and concepts, to treat physical phenomena that are quite diverse and have, at ﬁrst glance, little in common. Therefore, it is not surprising that in the articles devoted to phonons, magnons, excitons, and to electrons or polarons as well, we ﬁnd very similar equations and conclusions. The universality of the physical language reﬂects the unity of Nature itself. The passage to the study of highly excited states of a material led to the creation of the nonlinear dynamics of solids. New contributions to the lexical reserve of the language of solid state physics originated from nonlinear dynamics. For example, the concepts of topological and dynamic solitons were put forward, dynamic solitons appearing in solid state physics as a new type of collective excitation of a condensed medium. Not all parts of solid state physics are presented here with the same completeness and the same amount of detail. The branches reﬂecting the scientiﬁc interests of solid state physicists from the Ukraine and other former Soviet Union republics are the most extensively described. Although general problems of solid state 1

This is the title of the book in Russian (Editor’s note). xv

xvi

INTRODUCTION

physics are less systematically presented, the following areas are covered rather deeply and broadly: physical properties of metals, including superconductivity, electrical and optical properties of semiconductors and insulators, magnetism and magnetic materials, mechanical properties of crystals, and physics of disordered systems. One may also notice an emphasis on the applied physics of plasticity and strength. This is because of the fact that, although physics is an objective international science, some of its presentations or overviews found in textbooks, monographs, or encyclopedic publications unintentionally introduce subjective ideas and personal preferences of authors. The Dictionary includes articles reﬂecting the latest achievements in solid state physics, sometimes with results that have not yet appeared in monographs. This relates both to experimental discoveries and theoretical ideas. There are articles on high-temperature superconductivity, the quantum Hall effect, Kosterlitz– Thouless phase transitions in two-dimensional systems, autowave processes, fractals, etc. Novel nontraditional materials and techniques for investigation are described: amorphous substances, liquid crystals, quasi-crystals, polymers, low-dimensional systems, etc. In addition let us point out to the reader the “quantum-mechanical emphasis”, which may be noted in many articles devoted to diverse macroscopic phenomena and properties of solid bodies. Traditionally, use is made of the point of view that the quantum statistics of quasi-particles undoubtedly deﬁnes such macroscopic low-temperature properties of crystals as speciﬁc heat and thermal conductivity, electrical conductivity and magnetism. However, some authors only assign to quantum mechanics the role of describing microscopic laws explaining the dynamics of atomic particles. The discovery of high-temperature superconductivity transferred the quantum manifestations of particle dynamics into the region of moderately high temperatures. State-of-the-art experimental techniques make it possible to observe a number of phenomena involving macroscopic quantum tunneling. Thus, macroscopic solids fairly often exhibit some particular quantum features. Finally let us stress the role of models in solid state physics. As is well known, a model is a much simpliﬁed speculative scheme which allows a researcher, on the one hand, to propose a simple qualitative explanation of a property or phenomenon under study, and, on the other hand, to give a quantitative description of properties and to perform a complete theoretical calculation of characteristics of the phenomenon being studied. Models are utilized very often in solid state physics. Apparently, the most ancient model is that of an “absolutely solid body”. The model of perfect gas of quasi-particles is frequently employed; Ising’s model is well known in the study of magnetism. The model of a two-dimensional lattice of classical spins in the theory of phase transitions proposed by Onsager allowed him to give the ﬁrst statistical description of second-order phase transitions. The Frenkel–Kontorova and Peierls models are widely used in dislocation theory. References to them can be found in many of the articles included in this work. The need for this publication arises from the recent tremendous progress in this ﬁeld of physics, especially by the extension of its areas of practical applications. There have appeared new ﬁelds of electronics (optical electronics, acoustoelectronics); semiconductor electronics has changed and now employs an increasingly wider range of complex structures such as metal–insulator–semiconductor devices and computers with superconducting elements (cryotrons); and memory elements based on new physical principles have been developed. There are many promising new solid state materials based on garnets, rare-earth metals, magnetic semiconductors, amorphous metals, semiconductors, and, ﬁnally, the discovery of high-temperature superconductors in 1986. The compilers of this Dictionary hope that this publication will be useful for researchers working in solid state and other ﬁelds of physics (nuclear physics, plasma physics, etc.) and also for a wide audience of other readers, including, but not limited to, engineers investigating and utilizing solids, as well as doctoral and advanced students at universities. V.G. Bar’yakhtar A.M. Kosevich

HOW TO USE THE ENCYCLOPEDIC DICTIONARY In this Dictionary, we follow standard fundamental rules generally adhered to in encyclopedic publications. 1. Articles are arranged alphabetically; if a term (typeset in boldface) has a synonym, then the latter is given in the entry after the main meaning of the term (after comma, in usual print). 2. Some terms in the titles of articles adopted from other languages are followed by a brief etymological note (with clear abbreviations: abbr., abbreviated, fr., from; Gr., Greek; Lat., Latin; Fr., French; Germ., German, etc.). 3. The names of scientists appearing in the title or text of an article are commonly followed by the date of obtaining the result (effect, phenomenon) under consideration. 4. We use a system of cross-references (in Helvetica italics) to other articles. Additional terms explained within the same article are typeset in Times italic and, together with the main entries, are listed in the Subject Index at the end of Volume 2. Many terms synonymous to those in the article titles may be also found in this Subject Index. 5. Units of physical quantities and their symbols are given in the systems of units most commonly used in solid state physics. For the relations which convert these units into SI, see the tables included in the article Units of physical quantities. 6. The ﬁgures are explained either in their captions or in the text of the article. 7. Usually, the notation used in formulae is explained in the text of that article. However, some symbols have the same meaning throughout the Dictionary (unless otherwise speciﬁed): c, speed of light; h and = h/2π , Planck constant; T , absolute temperature; kB , Boltzmann constant; λ, wavelength; ν and ω = 2πν, frequency. The notation of some elementary particles is also standardized: ν, photon and gamma quantum; e, e− , electron; p, proton; n, neutron; d, deuteron; π and π ◦ , pions; μ± , muons; K ± and K ◦ , K-mesons.

xvii

This Page Intentionally Left Blank

Aa ABLATION (fr. Lat. ablatio, removal, taking away)

ABRIKOSOV–SUHL RESONANCE (A.A. Abrikosov, H. Suhl, 1965) The abnormal increase of the electron spin- ip scattering amplitude of conduction electrons on a

The removal of mass from the surface of a solid brought about by a heated gas ﬂow sweeping past it.

paramagnetic impurity when the energy ε of the scattered electron approaches the Fermi energy εF of the metal. The cause of the Abrikosov–Suhl resonance is the creation of a long-lived bound state of a conduction electron with a paramagnetic impurity due to the indirect interaction of conduction electrons with each other via the impurity spin when the spin–paramagnetic impurity exchange interaction constant is negative, i.e. J < 0. The Abrikosov– Suhl resonance manifests itself below the Kondo temperature T K by an anomalous temperature dependence of the behaviour of the resistivity and the magnetic susceptibility of a metal (see Kondo effect). The expression for the resistivity of a metal is derived by the selective summation of the “dangerous” terms of the perturbation expansion in the parameter |J |/εF 1 (diagrams calculated in the so-called parquet approximation), and has the form −2 εF J ν(εF ) (0) , ln ρ = ρs 1 + n kB T

This is observed during the motion of material bodies and space crafts through the atmosphere at high velocities. Ablation occurs as a result of erosion, melting, and sublimation. It is used to cool key parts of super- and hypersonic aircrafts, spacecrafts, and rocket engines by coating them with layers of an ablatable material (e.g., ceramics, or pyrolytic graphite). The ablation material must have high melting and sublimation temperatures and a large speci c heat.

ABRASIVE MATERIALS, abrasives (fr. Lat. abrasio, scraping)

Fine-grained solid materials intended for working (polishing, ﬁnishing) a material surface. The working consists in cutting and scraping the surface by a great number of randomly oriented sharp edges of abrasive grains. Typical abrasive materials are diamond (natural or synthetic), carborundum, the cubic modiﬁcation of boron nitride, and boron carbide. Abrasive materials are characterized by hardness, strength, granularity (describing the magnitude and dispersion of the grain size); knowing these parameters permits the selection of abrasive materials for particular purposes, and provides the expected precision of the working. Depending on their relative abrasive abilities, abrasive materials can be classiﬁed in terms of the following scale: diamond (1.00), cubic boron nitride (0.78), boron carbide (0.60), silicon carbide (0.50), and titanium carbide (0.42).

(0)

where ρs

is the resistivity calculated in the ﬁrst

Born approximation, ν(εF ) is the conduction density of electron states at the Fermi energy, and n is

the metal density. The denominator vanishes at the Kondo temperature εF n . exp − TK = kB |J |ν(εF ) In the temperature range T TK , perturbation theory is no longer valid, and a more detailed analysis shows that a spin complex of a conduction electron with an impurity is created, where at 1

2

ABRIKOSOV VORTICES

T = 0 the impurity spin is shielded by the conduction electrons. In the vicinity of TK the spin parts of the thermodynamic and kinetic characteristics of a metal sharply change their temperature dependences, remaining ﬁnite over the entire temperature range. The exact solution of the Kondo problem was obtained by P. Wiegmann and N. Andrei (1980). ABRIKOSOV VORTICES, vortex laments (A.A. Abrikosov, 1956) Vortex current structures of type II superconductors in magnetic ﬁelds with strength higher than the lower critical eld Bc1 (T ), but lower than the upper critical eld Bc2 (T ), i.e. in the domain of the mixed state (see also Shubnikov phase).

First predicted theoretically and then observed experimentally Abrikosov vortices are topologically stable singlet states, involving the penetration into a superconductor of minimal magnetic ﬂux quantities, equal to the ﬂux quantum Φ0 (see Quantization of ux). One can think of these vortices as quantum “rods” of magnetic ﬂux encircled by superconducting current ﬂow and pierced by magnetic ﬁeld lines (Fig. 1). For an isolated

Fig. 1. Abrikosov vortex. The arrows show the direction of the supercurrent ﬂow. The normal phase core region is cross hatched. The coherence length ξ and penetration depth λ are indicated.

Fig. 2. Behaviour of the order parameter Δ and the magnetic ﬁeld strength B in the region of an isolated vortex. Within the core (r < ξ ) the order parameter |Δ| decreases rapidly, reaching zero at the center.

Abrikosov vortex, the outer diameter has a radius equal to the London penetration depth λL (see Penetration depth of magnetic eld), and inside there is a core of radius equal to the coherence length ξ , in which superconductivity is suppressed by the high density of encircling shielding current that supports the magnetic ﬁeld (Fig. 2). One circuit around the vortex axis changes the phase of the order parameter Δ by 2π . The magnetic ﬁeld is able to penetrate the superconductor in the form of vortices because of the negative surface energy of the N–S boundary in a type II superconductor. When an externally applied magnetic ﬁeld B is present there is a gain in energy via the formation of a microscopic inhomogeneous region with a maximal surface. The extent of the splitting is determined by the ﬂux quantization condition, whereby the minimal domain size pierced by the magnetic ﬁeld has the value (Φ0 /B)1/2 . Since this minimal size cannot be smaller than ξ , it leads to the limitation that superconductivity is only possible for magnetic ﬁelds smaller than the value Bc2 = Φ0 /2πξ 2 (upper critical ﬁeld). In an ideal type II superconductor, Abrikosov vortices arrange themselves in a triangular lattice due to their mutual repulsion (see Vortex lattices in superconductors). When transport current ﬂows perpendicular to the magnetic ﬁeld direction Abrikosov vortices can drift in the direction perpendicular to J and B due to the Lorentz force J × B, which causes the appearance of electrical resistance in the superconductor (see Resistive state). For a resistanceless supercurrent to ﬂow in a superconduc-

ABSORPTION OF ELECTROMAGNETIC WAVES

tor (called a hard superconductor) the Abrikosov vortices should be held in position by pinning sites or defects of the crystal lattice (see Kosterlitz– Thouless transition, Vortex pinning). ABSOLUTE DIAMAGNETISM, ideal diamagnetism

The state of a superconductor in which a magnetic ﬁeld is completely excluded from its interior at a temperature below its critical temperature Tc . This occurs when the applied magnetic ﬁeld B is lower than the thermodynamic critical magnetic e ld Bc (T ) for a type I superconductor, and lower than the lower critical eld Bc1 (T ) of a type II superconductor (see Meissner effect). This implies that in the superconducting state the magnetic susceptibility χ attains its highest negative value χ = −1 in SI units (χ = −1/4π in Gaussian units). Absolute diamagnetism is caused by the persistent supercurrents which circulate in the outer surface layer of the material and shield the interior from the penetration of magnetic ﬂux (see Penetration depth of magnetic eld). This diamagnetism results in repulsion between a superconductor and a magnet, and the levitation of a magnet above a superconductor. Absolute diamagnetism is utilized in the manufacture of frictionless bearings, and the operation of trains levitated above their tracks. ABSORPTION (fr. Lat. absorptio, suck)

Absorption is the uptake or extraction of ingredients dissolved in or mixed with the bulk of a gas or liquid by another solid or liquid material called an absorbent. Absorption is one of the cases of sorption. In contrast to the surface process of adsorption, absorption occurs in the bulk of the absorbent. Absorption can be complicated by the chemical interaction of the absorbing substance with the absorbent (chemisorption). Absorption is used in industry to separate the components of a gas mixture by selective absorbents, possibly obtaining them in pure form by desorption with absorbents that can be reused afterwards. Examples are (1) the absorption of butadiene during the manufacturing of synthetic rubber; (2) removing gases from harmful admixtures (e.g., H2 S, SO2 , CO2 , CO); (3) obtaining a gas product such as sulphuric acid by absorption of SO3 ,

3

(4) the extraction of hydrocarbon gases (natural and synthetic) from their mixtures (e.g., propanes, butanes and pentanes). ABSORPTION COEFFICIENT, absorption factor, absorptance, absorptivity

The ratio of energy (particle) ﬂux, absorbed by a given sample, to the incident ﬂux. The term “absorption factor” is sometimes used in reference to an absorption index that is deﬁned as the natural logarithm of the reciprocal of the absorption factor. ABSORPTION EDGE See Intrinsic light absorption edge. ABSORPTION INDEX

A quantity α, which is the reciprocal of a distance, by which radiation ﬂux in a parallel beam is attenuated by the factor of 1/e as a result of its absorption by the material (cf. Absorption coef cient). It is introduced to characterize radiation intensity I = I0 e−αx which decays exponentially with the distance (see Beer–Lambert law). The value of the absorption index in crystals may depend on the direction of propagation, and the type of polarization of the radiation (see Dichroism of crystals, Pleochroism). ABSORPTION, LOW-FREQUENCY See Low-frequency enhanced magnetic resonance absorption. ABSORPTION, NONRESONANT See Nonresonance absorption. ABSORPTION OF ELECTROMAGNETIC WAVES in superconductors

The decrease in intensity of radiation, which is due to the partial transfer of radiation energy to the normal vibrations in the superconductor and, ﬁnally, to the crystal lattice. The rate of absorption of electromagnetic energy by a unit surface area of a superconductor is proportional to the active component of its surface impedance. At T = 0 the absence of this electromagnetic wave absorption exhibits a frequency threshold, i.e. it exists for ω Δ (where Δ is the energy gap), when an electromagnetic ﬁeld quantum possesses

4

ABSORPTION OF LIGHT

enough energy to break a Cooper pair. Measuring this threshold is one of the methods for determining Δ. In the mixed state of type II superconductors the absorption of electromagnetic waves is related to energy dissipation in the lattice of Abrikosov vortices and their viscous motion. In this case the measurement of electromagnetic absorption allows one to determine the magnetic ﬂux resistance and the so called pinning frequency. In electromagnetic ﬁelds of high amplitude nonlinear effects arise which are related to the probability of generating vortices by the wave ﬁeld, kinetic decoupling of Cooper pairs, and many-quantum absorption processes. ABSORPTION OF LIGHT See Light absorption. ABSORPTION OF SOUND See Sound absorption. ACCEPTOR

An impurity or structural defect with a local electronic level in the band gap of a semiconductor which can receive electrons from the valence band. An acceptor center is charged negatively if its local states are ﬁlled with electrons, and it is neutral if the states are empty. A predominance of acceptors over donors produces p-type conductivity (see Holes) with a temperature dependence determined by the height (typically 4π , the input

13

hypersound pulse splits into 2π -pulses. Acoustic self-induced transparency has been observed experimentally in dielectric and ferroelectric crystals, alloyed by paramagnetic ions of the iron group, satisfying the conditions of acoustic paramagnetic resonance at liquid helium temperatures. ACOUSTIC SOLID-STATE RESONATOR A device involving acoustic vibrations in a

mode close to that of a standing wave, viz. when the distance between the end plates of an acoustic resonator is an integral multiple of half-wave lengths. Typically, an acoustic resonator is made from a piezoelectric material (see Piezoelectricity), and the oscillations are excited by an electric ﬁeld. Piezoelectric acoustic resonators are electrical twopole and multipole elements with the impedance exhibiting resonant behavior near resonant frequencies. These resonators exhibit a high stability of the natural oscillation frequency, a longterm one of ∼10−6 –10−8 Hz, and a short-term one of 10−8 –10−10 Hz and higher. These are used to stabilize oscillator frequencies (of resonators), and form amplitude responses of ﬁlters (ﬁlter resonators). ACOUSTIC SPECTROMETER

An experimental installation for measuring sound absorption and sound velocity dispersion.

An acoustic spectrometer comprises the following basic components: a source of electromagnetic ultra-high frequency (UHF) oscillations, a component to pass on these oscillations to an acoustic wave transducer with a connection to the sample under study, a UHF section from the sample to the receiving end of the spectrometer, and a recording device. Acoustic spectrometers typically employ pulse and pulse-phase measurement techniques, those with continuous oscillations being less common. As a rule, the spectroscopic measurements determine the absorption and sound velocity dispersion as functions of external parameters such as magnetic ﬁeld, temperature, pressure, etc., at a ﬁxed UHF frequency. In pulse acoustic spectrometers, these quantities are the pulse amplitude and its traveling time through the sample under study, while in pulse-phase acoustic

14

ACOUSTIC SPECTROSCOPY

spectrometers the pulse that passes through the sample is compared to a signal coherent with it. The changes in amplitude and traveling time of the pulse through the sample are determined by beating the measured pulse with a reference signal. Pulse and pulse-phase acoustic spectrometers operate in both “transmission” and “reﬂection” modes. In the ﬁrst case, two acoustic wave transducers are placed on opposite sides of the sample, whereas in the second one, the same transducer is used for exciting and recording the acoustic oscillations. The pulse duration must be much less than its transit time through the sample. Continuous wave acoustic spectrometers operate in transmission only, and are used in measurements requiring low sensitivity to absorption factor variations. To increase the acoustic spectrometer response, use is made of low-frequency modulation of external parameters, with subsequent synchronous demodulation or digital accumulation of the signal. ACOUSTIC SPECTROSCOPY of solids

A collection of methods for investigating the resonant and oscillatory effects induced by the interaction of acoustic oscillations with different subsystems (electron, nuclear, spin, etc.) in a solid. Acoustic spectroscopy of normal metals. The acoustic spectroscopy of pure metals in external magnetic ﬁelds at low temperatures is the most diverse case since a large number of non-damping low-frequency collective waves can exist in metals. Owing to the cyclotron character of conduction electron motion and its interaction with acoustic waves in pure metals at low temperatures, the oscillating and resonant features of the sound absorption and the sound velocity dispersion depend on the external magnetic ﬁeld. If the conditions kl, Ωτ 1 are met (l, τ are the length and time of the mean free path of conduction electrons, k is the wave vector of the acoustic wave, and Ω is the electron cyclotron frequency), one can observe a magnetoacoustic effect whereby particular electrons most effectively interact with the sound, as indicated by the magnitude and direction of the constant magnetic ﬁeld relative to k, and by the value of parameter ωτ (ω is the frequency of the sound wave). Particular phenomena appear, such as giant quantum oscillations of sound absorption

and velocity dispersion, geometrical resonance, acoustic cyclotron resonance, Doppler-shifted cyclotron resonance, coupled acoustic and electromagnetic waves. These magnetoacoustic effects can provide extremum cross-sections, Fermi surface geometry, cyclotron masses, Fermi velocities and other energetic and kinetic parameters of conduction electrons (see also Electron–phonon interaction, Electromagnetic generation of sound, Acoustic wave ellipticity, Rotation of acoustic wave polarization plane). Acoustic spectroscopy is also an effective technique for studying an energy gap and its dependence on temperature and crystallographic direction. Acoustic spectroscopy of paramagnetic centers in insulator and semiconductor crystals is based on the application of hypersound waves for investigating the electron energy spectrum structure and the electron–phonon interaction of paramagnetic centers based on hypersound acoustic paramagnetic resonance (APR) spectroscopy. The resonant absorption of hypersound corresponding to APR in dielectric or semiconductor crystals containing paramagnetic centers is associated with induced transitions between the levels of the electron paramagnetic centers’ energy spectrum, and the APR line intensity (resonant absorption value) is proportional to the electron–phonon coupling of the center. That is why the APR characteristics such as the resonant magnetic eld and line width, as well as their dependence on the temperature, relative orientation of the magnetic ﬁeld and crystallographic directions, yield direct and accurate data on the positions of the ground and excited energy levels of the paramagnetic center, and its interaction with selected crystal lattice vibrations (electron–phonon interaction). Hypersound APR spectroscopy is an effective technique for studying the energy spectrum of non-Kramers centers with forbidden magnetic-dipole transitions and, especially, paramagnetic centers with orbital degeneracy in cubic crystal e lds, involving a strong electron–phonon–ion interaction. Acoustic spectroscopy of magnetically ordered crystals. These crystals exhibit elementary excitations of magnetization, such as magnons or spin waves. The magnetic subsystem energy is determined by the electric (exchange) and magnetic (dipole–dipole and spin–orbit) interactions

ACOUSTIC WAVE AMPLIFICATION

which depend on the distances between atoms. Magnons interact with phonons and undergo mutual scattering. This interaction is especially pronounced at crossings of magnon and phonon spectral branches in the region of magnetoacoustic resonance. In this case, coupled magnetoelastic waves having the amplitude equally dependent on the magnetization and elastic strain propagate in the crystal. Hypersound investigations of magnetoacoustic resonance, which underlie acoustic spectroscopy of magnetically ordered crystals, provide direct data on the structure of the magnon spectrum. One measures the resonant absorption value and the hypersound velocity change in a magnetic ﬁeld as a function of the temperature for several relative orientations of the external magnetic ﬁeld and the crystal. Acoustic spectroscopy is highly effective for the study of phase transitions in magnetically ordered crystals. ACOUSTIC SPIN ECHO

Coherent acoustic response of an electric or nuclear spin system in a paramagnetic crystal to the application of an acoustic or acousticoelectromagnetic pulse sequence during its resonant interaction with a spin system. Through the spin–phonon interaction (see Spin Hamiltonian), the acoustic pulse creates an inphase precession of dipole moments or quadrupole moments which, after the end of the pulse, become dephased in the time T2 under the inﬂuence of relaxation processes. If the excitation pulse length is less than T2 , the spin system dynamics is independent of the excitation ﬁeld amplitude at that given time, but it is determined by its value in the preceding period. Therefore, the application of the second pulse after the time τ < T2 causes the reversal of the dephasing process so that the initial phased state is recovered after the time interval 2τ (so-called phase memory effect). In materials with a strong spin–phonon interaction acoustic oscillations are generated (acoustic echo-response) at the moment of full phasing, in addition to the generation of electromagnetic ﬁeld pulses. Acoustic spin echo is the acoustic analogue of the magnetic resonance spin echo and photon echo. Acoustic spin echo enables one to measure the relaxation time and the spin–phonon interaction. Spin memory accounts for such nonlinear effects as acoustic selfinduced transparency and induction.

15

ACOUSTIC VIBRATIONS of crystal lattice

A type (branch, mode) of small oscillations of crystal atoms, when a displacement of the center of mass of a unit cell occurs; sometimes they are

called translational vibrations. The dispersion law (the dependence of the frequency ω on the wave vector k) of acoustic vibrations for small values of k is linear: ω = vph k, where vph is the phase velocity of the atomic displacement waves. It is an ordinary sound wave (hence the term “acoustic branch”), i.e. a matter density wave with frequency 0–1013 s−1 . At high frequencies, the dispersion law becomes nonlinear. In a three-dimensional crystal, there are always three branches of vibrations: with k directed along the symmetric direction in the crystal, one longitudinal and two transverse modes exist (the same as for an elastic-isotropic medium), the displacement vectors in transverse waves being mutually perpendicular. The quanta of vibrations are referred to as acoustic phonons. See also Crystal lattice dynamics and Phonons. ACOUSTIC WAVE AMPLIFICATION by current carrier drift

An effect which is the reverse of the electronic attenuation of acoustic waves. Ampliﬁcation of acoustic waves by charge carrier drift occurs in semiconductors and layered structures of the piezodielectric-semiconductor type when the drift velocity of free current carriers exceeds the phase velocity of the acoustic wave. For this ampliﬁcation to occur the acoustic waves must interact with free charge carriers. The strongest and most extensively studied interaction mechanisms are those involving the piezoelectric effect (see Piezoelectricity) and the strain potential. The piezoelectric interaction is dominant in piezosemiconductors at low frequencies ( v s , the electron absorption coefﬁcient becomes negative, and for l/λ 1 it is given (in cm−1 ) by K 2q ωτM (1 − vd /vs ) , 2 ω2 τ 2 (1 − vd /vs )2 + (1 + q 2 r 2 ) M D (1) where K is the electromechanical coupling constant for the given direction of wave propagation, τ M is the Maxwell relaxation time, r D is the Debye screening radius, ω is the wave frequency, and q = 2π/λ. Eq. (1) provides, for the most part, an adequate description of experiments on acoustic wave ampliﬁcation in piezosemiconductors which exhibit moderate electron mobility: CdS, CdSe, ZnO, GaAs, etc. (μ = 50–5500 cm2 ·V−1 ·s−1 ). The general nature of the relation between the electron absorption coefﬁcient and the drift velocity is shown in Fig. 2. Experimentally obtained electron ampliﬁcation coefﬁcients are of the order of tens and even hundreds of dB/cm. The nature of the interaction changes with increased frequency and with increased mean free path of the carriers. As the wavelength approaches the carrier mean free path the energy exchange between free carriers and the waves ceases to be dependent on collisions. In the case of a purely αe =

Fig. 1. Phase relationships between potential wave oscillations (solid lines) and electron concentration oscillations (dashed lines) for three successive times (a), (b) and (c).

at wavelength λ undergo a large number of collisions. Due to momentum relaxation, the motion of electrons with the wave is not inertia-free: as a result, the peak values of the electron concentration lag behind the potential minima, and the majority of grouped electrons become located at those positions of the charge pattern where the wave ﬁeld accelerates electrons in the wave propagation direction (see Fig. 1(a)). As this takes place, the energy of the wave is transferred to electrons, and the wave decays. The generation of a current carrier drift in the wave propagation direction in a semiconducting crystal brings about a change of the value of the absorption. Once the drift velocity v d equals the acoustic wave velocity v s , the concentration maxima coincide in space with the negative potential peaks, and the electron absorption discontinues because the wave no longer expends energy on inducing electron transport (Fig. 1(b)). When v d > v s , the peak values of electron concentration are ahead of the negative peaks of the potential (Fig. 1(c)). The electrons, which had been accelerated by the drift ﬁeld are now decelerated by the alternating wave ﬁeld. The energy, which is acquired by electrons from the electron drift genera-

Fig. 2. Dependence of the absorption coefﬁcient α on the ratio v d /v s of the electron drift velocity to the wave velocity for the two limits ql 1 (curve) and ql 1 (straight line). Note that for both limits at v d = v s the coefﬁcient α changes sign.

ACOUSTIC WAVE ELLIPTICITY

collisionless interaction (l/λ 1), the energy exchange with the wave involves only those carriers (e.g., electrons), which exhibit the projections vT x of the thermal velocity on the wave direction x close to the acoustic wave velocity (see Landau damping). The role played by the remaining electrons is limited to shielding the wave piezoelectric potential. In the process of energy exchange, the carriers characterized by vT x < v s gain energy from the wave, whereas those of vT x > v s give up energy to the wave. In the absence of drift, as well as at 0 < v d < v s (or under the conditions of back drift), most of the carriers belong to the former group (i.e. exhibit vT x < v s ), and hence the wave is attenuated. Under supersonic conditions favoring the drift of carriers (v d > v s ), the electron velocity distribution exhibits a distinguishing inversion, namely, the electrons that give up their energy to the wave exceed the number of those that gain energy, and hence the sound wave is ampliﬁed. The energy of the source of the drift ﬁeld is transferred to the waves, and the electron absorption coefﬁcient (in cm−1 ) changes sign at v d = v s : √ 2 K 2 q π(vs /vT )q 2 rD vd αe = 1 − . (2) 2 vs (1 + q 2 r 2 )2 D

The ampliﬁcation coefﬁcient is a linear function of the drift velocity. The collision-free mode of interaction is easily observed in semiconductors featuring a high electron mobility, e.g., in n-InSb, at liquid-nitrogen and liquid-helium temperatures at sound frequencies 200–500 MHz. As the frequency increases (10 GHz), the piezoelectric coupling mechanism gives way to the strain-potential mechanism, which occurs in all semiconductors, not only in piezoelectric ones. At high frequencies and low temperatures the electron de Broglie wavelength in certain semiconductors becomes comparable to the sound wavelength. In this case quantum effects are of considerable importance in the acousto-electronic interaction. These effects manifest themselves in certain features of the screening of the electric ﬁeld, and the attenuation and “shutdown” of acousto-electronic ampliﬁcation at q 2p, where p is the Fermi momentum or thermal momentum, depending on the electron statistics used. The effect of ampliﬁcation of acoustic waves by

17

charge carrier drift may be utilized in acoustoelectronic ampliﬁers, which are the solid-state analogues of travelling-wave tubes. These devices convert a signal into an acoustic form, amplify it, and then convert it back into electromagnetic oscillations. The advantages of acoustoelectronic ampliﬁers are low values of mass and overall dimensions. These devices, however, are not free from serious drawbacks, such as: high heat dissipation, high supply voltages, low efﬁciency, losses by energy conversion, high noise level, etc. Some of these disadvantages may be eliminated either fully or partially by application of ampliﬁers that operate by surface acoustic waves. The latter devices are based on laminated structures of a piezodielectric-semiconductor, the surface acoustic waves being initiated and propagated on the piezoelectric surface, which adjoins the semiconductor. The acousto-electronic interaction in laminated structures is induced by virtue of ac ﬁelds that penetrate from the piezoelectric into the semiconductor. Ampliﬁcation of acoustic waves by current carrier drift was ﬁrst observed by A.R. Hutson, J.H. McFee, and D.L. White (1961) in CdS crystals. ACOUSTIC WAVE CONICAL REFRACTION See Conical refraction of acoustic waves. ACOUSTIC WAVE ELLIPTICITY

Quantitative characteristic of an elliptically polarized acoustic wave. The magnitude (absolute value) of the acoustic wave ellipticity (ε) is the ratio of the semiminor to the semimajor axes of the ellipse along which an element of volume of the medium of a propagating sound wave moves. The sign of the ellipticity indicates the direction of the motion. The limiting cases of ellipticity, namely ε = +1 and ε = −1, correspond to clockwise and counterclockwise circular polarizations while ε = 0 corresponds to a linearly polarized wave. The acoustic wave ellipticity is always accompanied by a rotation of the acoustic wave polarization plane. The acoustic wave ellipticity may be either related to the internal structure of the medium, or be due to the interaction of the matter with a magnetic ﬁeld (see Acoustic analog of Faraday effect, Acoustic analog of Cotton–Mouton effect, Rotation of acoustic wave polarization plane).

18

ACOUSTIC WAVE FOCUSING

ACOUSTIC WAVE FOCUSING Concentration of the sound energy in a small region by the formation of a convergent wave front.

acoustic channels in space, and increasing the efﬁciency of the non-linear wave interaction.

In an isotropic medium the convergent wave fronts are portions of spherical and cylindrical surfaces. The minimum sizes of focused regions are of the order of the sonic wave length. Focusing is used for its local effect in small regions of space in the medium under investigation. Acoustic lenses and reﬂectors of corresponding shape may be used as focusing elements.

ACOUSTIC WAVE REFRACTION

ACOUSTIC WAVEGUIDE

A region of a medium relatively small in crosssection compared to its length, which localizes acoustic wave energy for the transmission and processing acoustic signals. The energy localization inside the wave-guiding structure is inﬂuenced by the acoustic nonuniformity of the medium. In the case of a smooth nonuniformity, the velocity proﬁle of an acoustic plane wave must have a minimum inside the structure in order to focus acoustic waves into the waveguide, taking into account wave front curvature. In the case of a sharp nonuniformity of the acoustical properties at the boundary, almost all the energy is localized inside the waveguide, and is retained there owing to the repeated reﬂections from the boundaries. The interference of the waves produces a complicated ﬁeld pattern in the waveguide arising from the superposition of normal modes of acoustic oscillations. Most widespread are planar acoustic waveguides which are inhomogeneous structures on the surface of substrates: strip waveguides formed from applied strips of another material, topographic waveguides involving grooves and ridges etched on the substrate, and diffusion waveguides wherein the inhomogeneities arise from the implantation of impurities in the substrate. There are also ﬁber acoustic waveguides. Distinctive features of the waveguide propagation are the presence of many acoustic vibration modes with strong dispersion. The latter is widely used for the development of dispersion devices for acoustic signal processing: ultrasonic delay lines, ﬁlters, waveguide lenses. The pronounced energy localization inside a waveguide enables the directing and transmitting of acoustic signals: without loss from the wave divergence, multiplexing

Variation of the direction of wave propagation in a nonuniform medium caused by the dependence of the phase velocity on the coordinates. The term “refraction of acoustic waves” refers to cases where geometrical acoustics is applicable, and it means the refraction of sonic beams at a planar or smoothly bent (on the scale of wavelengths) interface between two media. In the medium with a continuous dependence of the phase velocity on the coordinates the beam direction varies continuously, which involves refraction of waves. At the interface between two anisotropic media (see Bulk acoustic waves, Elastic modulus tensor) one incident plane harmonic elastic wave in the general case excites three waves – one quasi-longitudinal and two quasi-transverse refracted, and three reﬂected waves (see Re e ction of acoustic waves). The wave vectors of all these waves lie in the plane of incidence, determined by the normal to the interface and by the incident wave vector. In anisotropic cases refraction of the wave vector in the reﬂection of energy (sonic beam) from the interface can also occur (see Group velocity). ACOUSTIC WAVE ROTATION See Rotation of acoustic wave polarization plane. ACOUSTIC WAVE SCATTERING in solids

The process of formation of weak additional sound waves, differing in their characteristics from the incident wave, as a result of acoustic diffraction in a medium with inhomogeneities or obstacles. The process of scattering may be either coherent or incoherent, depending on whether the frequency of the vibrations is conserved or not during the scattering. In either case the scattering results in the attenuation of the sound wave. An example of incoherent acoustic wave scattering is the observation of hypersound in a dielectric crystal at low temperatures when the condition ωτ > 1 is satisﬁed (ω is the hypersound angular frequency, and τ is a thermal phonon lifetime). Absorption in that case is due to a three phonon scattering process whereby the incident phonon

ACOUSTO-ELECTRIC EFFECT

ﬂux forms a hypersonic wave of thermal phonons with long lifetimes, a result which arises from anharmonic vibrations of the crystal lattice. Irreversible absorption of the hypersound takes place, with the incident energy transferred to the thermal phonons. For coherent acoustic wave scattering off static inhomogeneities in a solid, scattered waves of the same frequency appear, with characteristics that depend on the type of incident wave, the inhomogeneities, and the boundary conditions at the surface. An example of such a coherent process may be found in the scattering of sound from crystalline inhomogeneities, such as the temperature-independent residual attenuation of hypersound in dielectric crystals at low temperatures. ACOUSTIC WAVE, SUBSURFACE See Subsurface volume acoustic waves. ACOUSTIC WAVE, SURFACE See Surface acoustic waves. ACOUSTIC WAVE TRANSDUCER

A device which transforms an electromagnetic vibration into acoustic ones, and vice versa. The majority of acoustic wave transducers are reciprocal, i.e. they may serve both as emitters and as receivers of acoustic vibrations. In ultrasonic and hypersonic investigations of bulk acoustic waves the most common transducers make use of the piezoelectric effect (see Piezoelectricity) or the phenomenon of magnetostriction. In resonance piezoelectric transducers, which have a thickness equal to an odd number of half wavelengths, monocrystalline quartz or lithium niobate (see Niobates) plates are used as operating elements at frequencies up to 1 GHz. Alternative materials are barium titanate, lithium tantalate, bismuth germanate, and piezoelectric ceramics. At frequencies in the UHF range the resonance acoustic wave transducers are applied at the samples under investigation, or at the sound wave guides in the form of thin lms of ZnO, CdS and other piezoelectric materials. The alternating electric ﬁeld is applied and recorded at the piezoelectric element either by the direct insertion of the latter into the electromagnetic circuit, or with the help of UHF

19

resonators or transmission lines. A thin magnetostriction transducer of acoustic waves is a magnetic lm applied at the end of the sample. The ﬁlm magnetized by an applied magnetic ﬁeld is deformed by the oscillating magnetic component of the UHF ﬁeld. Improved matching of the impedance of the acoustic wave transducer with the UHF guides and resonators may be achieved with the aid of piezoelectric transducers based on the depletion layers of piezosemiconductors, formed with many-layered and many-element constructions. For the excitation and recording of surface acoustic waves one may employ counter-pin transducers, in which the distribution of the electromagnetic ﬁeld and the corresponding deformation at the sound guide surface is pregiven or ﬁxed. These acoustic wave transducers are also used for excitation and recording of volume modes, spread at an angle to the surface at which the transducer is placed. This mode of exciting volume oscillations is used in dispersion delay lines when the effect of the sound velocity dispersion is reﬂected by the passage through different distances of vibrations with different wave lengths. For measurements of the absolute values of crystal lattice vibrations capacitance transducers have found their wide application, with their design in the shape of ﬂat plate capacitors, one plate of which is rigidly connected with the sample. See also Phonon generation, Electromagnetic generation of sound. ACOUSTO-ELECTRIC DOMAIN

A stationary or moving region of strong electric ﬁeld and an elevated intensity of acoustic noise which forms in semiconductors as a result of the ampliﬁcation of thermal crystal lattice vibrations by the electric current at a charge carrier drift velocity faster than that of the sound (see Acoustoelectric effect). ACOUSTO-ELECTRIC EFFECT

Establishment of a constant current or electromotive force caused by the transfer of momentum and energy from a traveling ultrasonic wave to conduction electrons (see Acousto-electronic interaction). The capture of electrons by the local electric ﬁelds arising in the conductor under the action

20

ACOUSTO-ELECTROMAGNETIC EFFECT

of an ultrasonic wave leads to their being carried along in the direction of the sound propagation, and an acousto-electromotive force arises along the sample. When the sample is introduced into a closed electric circuit an electric current begins to ﬂow through it. The current density is jA.E. = −2μΓ I /v (G. Weinreich, 1957), where Γ is the coefﬁcient of sound absorption by the conduction electrons, I is the ultrasonic wave intensity, v is the sound velocity, μ = eτ/m is the mobility, τ is the mean free path time. As seen from the expression for jA.E. , the sign of the acousto-electric current or acousto-electromotive force EA.E. = jA.E. σ (σ is the conductivity) depends on the sign of Γ , and can change depending on the ultrasonic wave propagation direction, its damping, or its ampliﬁcation. During the propagation of a surface acoustic wave a transverse acousto-electric effect is observable. When a transverse acousto-electric current directed into the sample bulk arises along with the longitudinal one; this is linked with the wave localization on the surface. See also Acoustomagnetoelectric phenomena, Surface acoustic wave. ACOUSTO-ELECTROMAGNETIC EFFECT

The appearance of a magnetic moment in a semiconductor crystal under application of a sufﬁciently strong electric ﬁeld causing the ampliﬁcation of acoustic noise (phonons). The generated ﬂux of acoustic energy results in the movement of charge carriers (see Acousto-electric effect), and in some cases the charges may not move along the electric ﬁeld direction (e.g., in an anisotropic crystal where the direction of maximal noise ampliﬁcation may not coincide with that of the applied electric ﬁeld). As a result, a circular electric current begins to ﬂow around the sample, and hence the appearance of a magnetic moment. Acoustic energy ﬂux injected into a sample from outside can induce a magnetic moment in the absence of the external electric ﬁeld (acoustomagnetic effect). The nonlinearity of charge carrier motion is related both to the anisotropy of crystals, and the acoustic energy ﬂux nonuniformity. This phenomenon is also observable in metals. The acoustomagnetic ﬁeld arises, in particular, during the propagation of surface acoustic waves. In this case

the acting force ﬁeld is always nonuniform because the oscillatory displacement of the particles decays into the bulk of the sample. ACOUSTO-ELECTRONIC AMPLIFIER See Acoustic wave ampli cation. ACOUSTO-ELECTRONIC INTERACTION (AEI)

Interaction of acoustic waves with charge carriers (conduction electrons and holes in metals, semimetals and semiconductors). In metals, due to the Pauli’s principle, the interaction with acoustic waves (sound) involves only electrons with energies close to Fermi energy EF . There are two main mechanisms of AEI: (1) the deformation mechanism involves a change in periodic potential of the crystal lattice and a local change of the dispersion law of quasi-particles E(p) in the electron Fermi liquid, (2) the electromagnetic mechanism is due to forces exerted on the electrons by electric and magnetic ﬁelds arising from the displacement of ions during the passage of the ultrasonic wave. For longitudinal sound, the ﬁelds are electrostatic and are screened by free electrons (see Electric charge screening) to a great extent. This leads to renormalization (p) of the strain potential Λik = λik (p) − λik (p), where the angle brackets indicate averaging the bare deformation potential λik over the Fermi surface. The quantity Λik can be interpreted as a distinctive phonon electric-charge in the metal. During propagation of the transverse sound wave the electrons are affected by the vortex electric ﬁelds (see Acousto-electric effect). In an external magnetic ﬁeld B, an additional, so-called induction interaction of the electrons with the acoustic waves arises, its strength being e(v · [U × B]), where v is the electron velocity, and U is the ion displacement velocity. This interaction involves the additional parameter (qRL )−1 , where q is the wave vector of the sound wave, and RL = pF /eB is the electron Larmor radius. The induction interaction prevails over the deformation in sufﬁciently strong magnetic ﬁelds when qRL < 1. Besides, in the presence of a magnetic ﬁeld AEI leads to various magnetoacoustic effects, in which electromagnetic resonances, ballistic and collective effects add their characteristic features.

ACOUSTO-ELECTRONICS

The great difference between the electron and ion masses leads to the fact that the sound velocity is many times less than the Fermi velocity of the electrons. This circumstance (adiabaticity) plays an important role in the interaction of electrons with sound. Adiabaticity supports introducing the concept of electrons and phonons as weakly interacting quasi-particles, and makes it possible to neglect inertial terms (Stewart–Tolman effect) in the AEI energy. In pure metals with a long mean free path l (ql 1) the adiabaticity underlies the fact that only electrons with a velocity v almost perpendicular to the sound wave vector can effectively interact with the sound (autophasing effect). In semiconductors, the AEI is mainly determined by the strain interaction related to the local change in the band gap under the action of the strain arising when a sound wave travels through the crystal. In ionic crystals and semiconductors with a large number of charged impurity atoms in the lattice, the electromagnetic mechanism of AEI is also possible. In superconductors, the AEI at temperatures lower than critical temperature of superconductors differs in some features from the AEI in normal metals. Due to the Cooper pairing of electrons (see Cooper pairs), the phonon absorption probability decreases and, as a consequence, a sharp (exponential) decrease of the ultrasound absorption factor occurs. Besides, the Meissner effect precludes the electromagnetic mechanism of AEI. ACOUSTO-ELECTRONICS

A branch of electronics dealing with the effects of excitation and propagation of acoustic waves in condensed media, the interaction of the waves with electromagnetic ﬁelds and electrons, and the development of acousto-electronic devices based on these effects. The diversity of effects utilized in the design of acousto-electronic devices suggests the division of acousto-electronics into the high frequency (microwave) acoustics of solids (effects of excitation, propagation and reception of high frequency acoustic waves and hypersonic waves), acousto-electronics proper (interaction of acoustic waves with conduction electrons in the bulk and on the surface of solids, see Acousto-electronic interaction), and acousto-optics (interactions between

21

light and acoustic waves). Acousto-electronics was formed as an independent part of electronics in the decade of the 1960s with the start of intensive studies stimulated by the discovery of the acoustic wave ampli cation by conduction electrons in cadmium sulﬁde crystals. The rapid development of acousto-electronics was caused by the necessity to create simple, reliable and smallscale radio signal processing devices for radioelectronic equipment. At the present time acoustoelectronic devices perform the following signal transformations: (1) in time (delaying and changing the duration of signals), (2) in phase and frequency (frequency and spectrum conversion, phase shift), (3) in amplitude (ampliﬁcation, modulation), and (4) those involving more complicated functional transformations (coding and decoding, signal convolution and correlation). In some cases, the acousto-electronic methods of signal transformation are simpler (as compared, e.g., to electronic methods) and, sometimes, they constitute the only possible choice. The use of these devices is predicated on the low propagation velocity of acoustic waves (compared to that of electromagnetic waves), weak absorption of acoustic waves in crystals with a high acoustic Q-factor (quality factor), as well as favorable interactions of these waves with electromagnetic ﬁelds and electrons. In acousto-electronic devices, both bulk acoustic waves and surface acoustic waves (SAW) are used. The manufacture of these devices employs piezoelectric materials and laminated structures composed of piezoelectric and semiconductor layers. Many acousto-electronic devices convert high frequency electric signals into acoustic waves (acoustic wave transducers) to propagate in a sound guide and then be converted back again into a high frequency signal. Components used for excitation and reception of bulk acoustic waves are mainly piezoelectric transducers: piezoelectric plates (at frequencies up to 100 MHz) and ﬁlm transducers (at frequencies above 300 MHz), while those employed for the excitation and reception of a SAW are opposite-pin transducers. The ultrasonic delay lines operating in the frequency range from several MHz to several tens of GHz, as well as quartz resonators for the radio frequency generator stabilization (see Acoustic solid-

0.10 no 2300 0.01 –

3138 3488 3295 3808 1681 2640 2505 3100 1010 2270 0.0017 0.045 0.05 0.014 0.015 0.015 0.073 0.09 0.062 0.01 ST, x y, z x, 112◦ x, 6.7◦ [110], [111] [110] z, 74.4◦ [100] [110], 24◦ –

state resonator), are among the most widely used acousto-electronics devices for bulk waves. The most common are acousto-electronic devices based on the SAW due to small loss for wave excitation, the possibility of wave propagation control at any point of a sound guide (along the wave propagation path), and the feasibility for designing devices with controllable frequency, phase and other responses. Such devices include resonators on the SAW, which are used as narrow-band acousto-electronic ﬁlters and are also introduced into a generator circuit for its frequency stabilization; delay lines (for long signal delay in memory elements); various ﬁlters based on the SAW (e.g., band ﬁlters, matched ﬁlters); coding and decoding devices and so on. The interaction of acoustic waves with conduction electrons in semiconductors and laminated structures of the piezoelectric–semiconductor type leads to such phenomena as electron absorption or ampliﬁcation of acoustic waves, the acoustoelectric effect, and others. These effects are useful in acousto-electronic generators. The nonlinear effects arising under the interaction of acoustic waves in piezoelectrics, semiconductors, and laminated structures of a piezoelectric-semiconductor type ﬁnd wide use in signal convolution and correlation devices. The interaction of light and acoustic waves in condensed media forms the basis for the operation of acousto-optic devices (deﬂectors, modulators, ﬁlters etc.). They can be used to control the amplitude, polarization, and spectral content of optical radiation, as well as its propagation direction (see Acousto-optics). ACOUSTO-ELECTRONICS MATERIALS

Pb[(Mn1/3 Sb2/3 )0.08 Zr0.42 Ti0.50 ]O3

α-quartz, SiO2 Lithium niobate, LiNbO3 Lithium tantalate, LiTaO3 Lithium tetraborate, Li2 B4 O7 Bi12 GeO20 Bi1.2 Sr0.8 TiSi2 O8 Pb2 KNb5 O15 K2.98 Li1.55 Nb5.11 O15 Tl3 VS4 Pb0.91 In0.03 [Zr0.44 Ti0.53 (Li3/5 W2/5 )0.08 ]O3

Coefﬁcient of electromechanical coupling Orientation Material (name, formula)

Table 1. Physical characteristics of some acousto-electronic materials

Speed of sound, m/s

Existence of cut with zero temperature coefﬁcient of delay yes no yes no no yes yes yes yes no

Acoustic loss in air (dB) at 100 MHz 0.03 0.04 0.03 0.04 0.0145 0.03 0.05 0.05 0.95 0.10

Industrial product Industrial product Industrial product Laboratory product Industrial product Laboratory product Specialized laboratory product Specialized laboratory product Specialized laboratory product Industrial product (high temperature and pressure) Industrial product (high tempetature and pressure)

ACOUSTO-ELECTRONICS MATERIALS

Comments

22

Materials used to create working parts for the branch of functional electronics, which involves devices and systems for processing large and extra-large (order of gigabits) information ﬂows. The physical basis for the operation of such devices is provided by the interaction of space and surface acoustic waves of various types (Rayleigh, Gulyaev–Bleustein, Love, etc.) with electromagnetic radiation ﬂuxes at various frequencies – from 10 to 1011 Hz. The main physical characteristics of some important acousto-electronics materials are given in Table 1. Some layered systems for devices are based on surface acoustic waves,

ACOUSTOMAGNETOELECTRIC PHENOMENA

23

Table 1. Physical characteristics of some layered acousto-electronic materials Material

Coefﬁcient of electro-mechanical coupling

Dielectric constant

Attenuation (dB) at 1 GHz

Carrier mobility, cm3 ·V−1 ·s−1

Ideal material Lithium niobate, LiNbO3 Bi12 GeO20 Lithium tetraborate, Li2 B4 O7 Quartz, SiO2 Aluminum nitride on colorless sapphire Zinc oxide on silicon Cadmium sulphide on silicon Gallium arsenide on silicon Silicon (substrate)

>0.010 0.045 0.013 0.012 0.012 (0.010)

3), all the states are localized provided the following inequality holds: t < γ W,

γ ≈ 1,

(1)

where t is the mean tunneling amplitude, or a quantity proportional to it, the width of the conduction band that would be created for W t . The value of γ is determined numerically. In the Lifshits model, the disorder is not speciﬁed by the spread in the site energies, but by the randomly positioned short-range impurities. In this model, Anderson localization takes place when the mean free path decreases to the order of the de Broglie wave length. If condition (1) for complete localization is not satisﬁed then the states in the central region of the band are not localized, but the ones

59

close to the top and bottom of the band still are. In this case, the electron system is in the insulating state if the Fermi energy EF is lower than the threshold energy (see Mobility edge) Ec ≈ W , and it is in the conducting state, if EF > Ec . The electrical conductivity behaves in the close vicinity of the metal–insulator transition point as follows: σ ∼ (t − γ W )ν σ ∼ (EF − Ec )ν ,

or ν = 0.5.

(2)

If the random potential in which the electrons move changes only slightly on a scale of the order of the electron wavelength, then the quantum value of the critical index ν = 0.5 “works” in a very narrow region, whereas in a wider region near the critical point the index ν takes on the quasiclassical value 1.7 predicted by percolation theory. All the preceeding remarks concern ordinary three-dimensional systems. It has been proven that in the one-dimensional case an electron has only localized states for any value of the disorder parameter W . Apparently this is also valid in the twodimensional case, except for the only inﬁnitely extended state in the middle of the band. Closely related to Anderson localization are such phenomena as weak localization and mesoscopics, in which the interference of electron scattering processes by several impurities, although weak, still plays a signiﬁcant role. It should be noted that Anderson localization is described in the single particle approximation. At ﬁnite temperatures, the inelastic particle interaction becomes signiﬁcant and cancels Anderson localization. However, it can be shown that selflocalization takes place even in an ideal crystal if inequality (1) is satisﬁed, where the quantity W has the sense of a characteristic level difference at neighboring sites. In an ideal crystal, this difference of levels is not due to impurities, but to the intrinsic interaction of particles with one another. Autolocalization has been observed in studies of the diffusion of 3 He atoms in solid 4 He. See also Elementary excitation spectra of disordered solids. ANDERSON MECHANISM OF HIGHTEMPERATURE SUPERCONDUCTIVITY (P.W. Anderson, 1987) A mechanism of superconductivity in systems

with “resonating” valence bonds (RVB).

60

ANDERSON MECHANISM OF HIGH-TEMPERATURE SUPERCONDUCTIVITY

This magnetic mechanism of Cooper pairing involves a fundamentally new type of ordering for two-dimensional systems with an antiferromagnetic Heisenberg interaction (see Antiferromagnetism). Proceeding from the experimental data on the insulating (La2 CuO4 ) and conducting (La2−x (Ba, Sr)x CuO4 ) phases of lanthanum compounds, Anderson proposed several hypotheses regarding their properties, and a possible superconductivity mechanism of high-temperature superconductors. The presence of bivalent copper Cu2+ with one hole in the unﬁlled 3d-shell classiﬁes La2 CuO4 as a magnetic insulator adequately described by Hubbard’s Hamiltonian (see Hubbard model) with a strong intra-atomic Coulomb repulsion hindering the free motion of the carriers (holes), and causing their localization (Mott metal–insulator transition). The Mott–Hubbard insulator ground state with one electron (hole) per atom (half-ﬁlled band) is equivalent to Heisenberg’s antiferromagnet (see Heisenberg magnet) with one spin S = 1/2 per site. A second Anderson suggestion based on H. Bethe’s works on one-dimensional magnetic materials, as well as on L. Pauling’s chemical bond theory, matches with the essentially quasi-two dimensional character of the structure of superconducting cuprates. The suggestion means that under certain conditions quantum ﬂuctuations, even at T = 0, are able to completely destroy antiferromagnetic ordering in the CuO2 planes, so that the complete wave function of the ground state of an individual plane can be represented by a linear combination of the wave functions of “valence-coupled” pairs of the localized carriers: C{n, m} (αn βm − βn αm ), ΨRVB = {n,m}

|ΨRVB |2 = 1,

n,m

(1)

where n, m are the bidimensional site vectors, {n, m} represent all possible conﬁgurations with contributions determined by the coefﬁcients C{n,m} , and αn , βn are functions of “up” and “down” spin projections. In this state, the mean value of a spin at each site is zero, but the phase coherence is retained. The lowest excitations above the ground state (1), known as spinons, are dangling bonds or individual unpaired spins. The lat-

ter are the topological defects (kinks), their thermodynamically equilibrium number being determined by the temperature. The kink displacement corresponds to the “valence bond transfer” from one site to another, with no change in energy and no transfer of charge taking place. It is in this sense that the state (1) corresponds to “resonating valence bonds”, while spinons (S = 1/2) turn out to be neutral, zero mass fermions. The transition from the insulating RVB-state to the metallic one is caused by introducing new holes into the system (by doping or a change in stoichiometry). The “extra” (free) holes are coupled to a spinon forming a new charged Boseparticle called a holon. The motion of holons both inside and between planes, their scattering by spinons, and the phenomenon of holon conﬁnement determine the ﬁnite resistance in the normal metallic phase, as well as the attraction with the formation of holon Cooper pairs, thereby facilitating a transition to the superconducting state at temperatures on the order of Heisenberg exchange interaction constant. The holon gas does not undergo a Bose–Einstein condensation. There is a relationship between the wave function (1) and the condensate wave function of the Bardeen– Cooper–Schrieffer theory

ΨBCS =

+ + a−k↓ |0, uk + vk ak↑ k

|ΨBCS |2 = 1,

(2)

+ where uk , vk are coefﬁcients, and akσ (σ =↑, ↓) are Fermi creation operators of carriers from the vacuum state |0. The wave function (2), projected on the pairs and then transformed into real coordinate space, acquires the functional form (1). Another feature of the Anderson mechanism lies in the possibility of a qualitative description of some unusual properties of high-temperature superconductors (such as the anomalous temperature dependence of the heat capacity, the resistance in the normal phase, anisotropy of conductance, etc.). Experiment shows that cuprate metal oxides in the normal state are ordinary Néel antiferromagnets. However, some arguments favor inducing the RVB-state in metal phases under conditions of strong spin interactions of free and localized carriers.

ANDREEV REFLECTION

ANDERSON MODEL (P.W. Anderson)

(1) In disordered systems theory – a strong coupling model with diagonal disorder described by Anderson’s Hamiltonian |nm| + εn |nm|, H =J n,m

n

where n, m are the sites of a d-dimensional lattice, n, m are pairs of the nearest neighbors, J is the transfer integral, and the energies εn at different sites n are independent, uniformly distributed random quantities. The pioneer work of Anderson gives arguments in favor of the fact that for d = 3, if εn are uniformly distributed in the interval [−W/2, W/2] and the quantity W/J exceeds some critical value (W/J )c , then all the states of this Hamiltonian are localized (Anderson localization). The Anderson model provides an effective analysis of the transition from quasi-Bloch (propagating) states to localized ones, and clariﬁes the presence and position of the mobility edge, characteristics of the ﬂuctuation elementary excitation spectra of disordered solids, and other properties of disordered solids. (2) In the theory of magnetism this approach provides a model Hamiltonian to describe the formation of the local magnetic moment of an impurity atom in a nonmagnetic metal as the impurity level changes relative to the Fermi level. The model admits an exact solution by means of the Bethe substitution (Bethe ansatz). (3) In the theory of metal-oxide superconductors – the model provides an explanation of resonating valence bonds (see High-temperature superconductivity, Anderson mechanism of hightemperature superconductivity). ANDERSON THEOREM (P.W. Anderson, 1959) A theorem stating that the electron scattering

by nonmagnetic impurities in superconductors has a slight effect on the critical temperature only. This theorem is based upon the invariance of the Hamiltonian with respect to time inversion. The Anderson theorem is not necessarily valid outside the framework of the Bardeen–Cooper–Schrieffer theory, namely, if one takes into account the weak localization of carriers, anisotropy of the Fermi surface, ﬁne structure of the density of electron states,

61

the presence of a dielectric gap on a part of the Fermi surface, etc. ANDREEV REFLECTION of quasi-particles (A.F. Andreev, 1964) A speciﬁc reﬂection of quasi-particles (electrons and holes) from the interface between the

superconducting (S) and normal (N) phases of a metal (NS-boundary).

During this process the quasi-momentum p of a reﬂected particle is conserved, but the signs of the charge and all three velocity components change. When an electron of energy ε (measured from the Fermi level) and velocity v = ∂ε/∂p is incident from the normal metal side on the NS interface, the reﬂected quasi-particle is a hole with the same energy ε and velocity v. The reﬂection of holes proceeds in a similar way. The value of the Andreev reﬂection coefﬁcient R depends on the quasi-particle’s energy: R(ε) = 1 for 0 < ε < Δ (Δ is the value of the energy gap in the superconducting phase); R(ε) → 0 for ε Δ. The essence of Andreev reﬂection is that at the NS-boundary the incident electron enters the superconducting condensate, forming a Cooper pair with an electron having the opposite momentum. A hole arising in the process moves back into the normal region. When the normal metal layer is situated between superconducting slabs (e.g., in the intermediate state of a superconductor or in SNS-junctions), Andreev reﬂection gives rise to distinctive quantization of the low-energy (ε < Δ) excitations of the N-layer (Andreev quantization). This quantization corresponds to a periodic motion of quasi-particles inside the N-layer, with the quasi-particle being an electron for half of the period and a hole for the other half. Andreev reﬂection manifests itself in a number of features of the thermodynamic and kinetic properties of the intermediate state of a superconductor. In particular, it leads to geometrical oscillation effects in ultrasonic attenuation, and to an additional thermal resistance of the intermediate state during thermal ﬂux propagation normal to N- and to S-layer, etc. As distinct from thermal ﬂux propagation, the passage of an electric current through the NS-boundary at low temperatures (kB T Δ) is not associated with overcoming the excess resistance of the S-boundary due to the quasi-particle

62

ANGULAR DEPENDENCE OF SPECTRA

reﬂection, since the conversion of the normal excitation current into that of Cooper pairs takes place under Andreev reﬂection. Andreev reﬂection has been directly observed experimentally in studies of the radio-frequency size effect, and of transverse magnetic focusing of electrons in NS-structures. ANGULAR DEPENDENCE OF SPECTRA of magnetic resonance The dependence of the resonant magnetic eld Br (in case of electron paramagnetic resonance, EPR) or resonance frequencies (in case of electron– nuclear double resonance, ENDOR; nuclear magnetic resonance, NMR) on the relative orientation

of the constant external magnetic ﬁeld B and the crystal axes, i.e. on the values of the polar angle θ and azimuthal angle ϕ that specify the B direction in a coordinate system relative to the crystal. The parameters of a generalized spin Hamiltonian are obtainable by comparing experimentally observed angular spectral dependences to those calculated from the Hamiltonian. Examining angular spectra in three mutually perpendicular planes permits determination of all parameters of the effective spin Hamiltonian (see Spin Hamiltonian para-

meters, Invariants), and the local symmetry groups of its interactions. An example of the angular dependences of the magnetic resonance spectra of the Gd3+ ion at a site of symmetry C2 is given in Fig. which plots the values of the resonant magnetic e ld Br versus the azimuthal and polar angles θ and ϕ, respectively, for the indicated transitions M → M − 1, where M is the eigenvalue of the projection of the electronic spin S = 7/2 on B. When the symmetry and arrangement of crystallographic axes (see Crystal symmetry) are unknown, they can be determined from EPR (NMR) spectra recorded for rotations around three mutually perpendicular axes ﬁxed in the crystal. In certain cases, the values of θ and ϕ also affect the line width and line intensity. An EPR spectrum is customarily called an anisotropic EPR spectrum, if the positions and intensities of its lines depend on the orientation of the sample relative to the external magnetic ﬁeld. For spin S 1 and in the absence of anisotropic hyper ne interactions, the anisotropic spectrum is observed only for centers belonging to non-cubic spin Hamiltonian symmetry groups, whereas in the presence of anisotropic hyperﬁne interactions

Angular dependence of EPR spectra of Gd3+ .

ANISOTROPIC MAGNETIC MATERIALS

with surrounding nuclei an anisotropic spectrum can be observed even for cubic symmetry groups. If the positions and intensities of EPR spectral lines are independent of the orientation of the sample under investigation relative to the direction of the external constant magnetic ﬁeld, then the spectrum is called an isotropic EPR spectrum. The concepts “anisotropic spectrum” and “isotropic spectrum” are valid also for other resonance phenomena such as NMR. ANGULAR MOMENTUM, moment of momentum

Vector product r × mv, where r is the position vector, v is the velocity of a material point of mass m. The angular momentum of an arbitrary system of points with masses mi , which move with velocities v i , is the sum of vector products

i r i × mv i , where r i is the position vector of the ith mass point relative to an origin of coordinates 0. The angular momentum depends on the choice of origin. ANHARMONICITY, VIBRONIC See Vibronic anharmonicity. ANHARMONIC VIBRATIONS of crystal lattices

Deviation from the simple harmonic nature of atomic vibrations in a crystal, i.e. a nonlinear relationship between the displacements of atoms (ions) from their equilibrium positions and the restoring forces. While the potential energy of a crystal in the harmonic approximation includes only terms of second order in the relative atom displacements, taking anharmonic vibrations into account leads to the appearance of cubic and higher order terms in the potential energy expansion in powers of the displacements. Anharmonicity of vibrations involves interaction between the normal modes (see Normal vibrations) of a harmonic crystal, which corresponds to taking into account both elastic and inelastic phonon collisions from the quantum point of view. Anharmonic vibrations are responsible for the thermal conductivity of insulators, the thermal expansion of bodies, the change in the dielectric function of the crystal with temperature, IR absorption and Raman scattering, etc. The anharmonic interaction of phonons leads to their scattering and decay which, in turn, determines the width (lifetime) and shift of the energy

63

levels. Accounting for the anharmonicity is a typical many-body problem, with its solution providing the answers to some fundamental questions of solid state physics, such as the possibility of forming two-phonon coupled states (biphonons), the role of soft modes in structural phase transitions, etc. Slightly and highly anharmonic crystals can be distinguished. Quantum crystals, systems with structural phase transitions, in particular ferroelectrics, fall into the latter type. The presence of solitons, which can contribute to the energy transfer and to the process of the restoring the equilibrium state after an external perturbation, is possible in an anharmonic crystal. ANISOTROMETER See Magnetic anisotrometer. ANISOTROPIC MAGNETIC MATERIALS Magnetic materials having different magnetic

properties along different directions. The most common anisotropic magnetic materials have one easy magnetization axis. Along this axis, high magnetization and low values of the coercive force are observed in soft magnetic materials and the maximal remanence is realized in hard magnetic materials. The magnetic anisotropy is natural for monocrystalline magnetics. The widely used polycrystalline anisotropic magnetic materials are obtained by a variety of methods. One of them is the production of crystallographic texture, i.e. preferable orientation of easy magnetization axes of individual crystallites along one common direction. Thus, in sheets of anisotropic electrical steel, the crystalline structure is produced by cold rolling and annealing, and in magnetically hard materials it is obtained by powder metallurgy which involves pressing in a magnetic ﬁeld. Another method of obtaining anisotropic magnetic materials involves producing magnetic texture by means of thermomagnetic treatment or thermomechanical treatment. In some anisotropic magnetic materials, both the crystallographic and magnetic texture are used simultaneously. Thus, e.g., the best magnetic properties are realized after thermomagnetic treatment of alloys of the alnico type, in which the columnar crystallographic texture is produced by directed crystallization.

64

ANISOTROPIC MEDIUM

ANISOTROPIC MEDIUM

A medium with some properties that depend on the spatial directions in it. Anisotropic media necessarily possess longrange order, involving translational and/or orientational order (see Long-range and short-range order). The natural anisotropy of crystals is related to the symmetry of the ordered arrangement of atoms (molecules) in space, and is the more pronounced, the lower the crystal symmetry. Many mechanical (anisotropy of elasticity, plasticity, hardness, etc.), thermal (thermal expansion and others), electric (electrical conductivity, dielectric constant, etc.), magnetic (magnetic anisotropy), and optical (birefringence) properties of monocrystals are anisotropic. Only a few crystal properties (e.g., density and speci c heat) do not depend on direction (isotropy). Ordinary liquids, in the absence of external factors, are isotropic like gases, due to the absence of long-range order in the relative positions and orientations of the constituent molecules (or atoms). The anisotropy of liquid crystals is due to the asymmetry and the long-range correlation of relative molecular orientations. The quantum liquid 3 He exists in two antiferromagnetic modiﬁcations: a highly anisotropic A-phase with weak ferromagnetic properties (in which superﬂuid motion is not always possible in some directions) and a weakly anisotropic B-phase. The inhomogeneity of a body in its surface layer results in local anisotropy of physical properties. Some chemical characteristics of a medium can also be anisotropic, e.g., the oxygenation and etching rates. The anisotropic properties of a medium can be characterized by corresponding tensor coefﬁcients (susceptibilities). ANISOTROPY FACTOR of a cubic crystal

This factor H = 2c44 + c12 − c11 depends on the elastic constants cij (see Elastic moduli). For an isotropic medium, H = 0 (see Isotropy). The anisotropy elasticity ratio deﬁned by A = 2c44 /(c11 − c12 ) has the value A = 1 for an isotropic medium. The quantity A can be either less than or greater than unity. For example, A has the values 1.00 for W, 1.21 for Al, 2.36 for Fe, 3.21 for Cu, and 0.69 for Cr. H is measured in Pa, and A is dimensionless.

ANISOTROPY FIELD See Magnetic anisotropy. ANISOTROPY, GROWTH See Growth anisotropy. ANISOTROPY, MAGNETIC See Magnetic anisotropy. ANISOTROPY OF CRYSTALS

Dependence of the physical properties of crystals on the direction.

The anisotropy is caused by the periodic arrangement of atoms in a crystal, and is related to the crystal lattice symmetry (see Crystal symmetry). Physical properties are the same only in equivalent crystallographic directions. According to the Neumann principle (see Crystal physics), the symmetry of any physical property cannot be lower than the symmetry of the point group of the crystal, but can be higher than that. Physical properties of crystals are described by tensors of rank from zero to four. Examples of properties described by a zero-rank tensor (scalar) are density and speci c heat (they are isotropic for every crystal). A ﬁrst-rank tensor (vector) describes, for instance, the pyroelectric effect, while thermal conductivity, thermal expansion and magnetic susceptibility are described by tensors of rank two. Tensors of third rank describe the piezoelectric effect (see Piezoelectricity) and electrooptical effect; most elastic properties of a crystal are described by a tensor of rank four. The symmetry of these properties depends on the crystal lattice symmetry. For crystals of low symmetry (triclinic, monoclinic), all these properties are anisotropic. Some of these properties for high symmetry crystals are isotropic, e.g., in a cubic crystal, all the properties described by a tensor of rank two are isotropic. ANISOTROPY OF ELASTICITY

Dependence of the elastic properties of a material on the spatial direction in it. The anisotropy of elasticity is characterized by the symmetry of its elastic modulus tensor, and by the values of its components. The elastic modulus tensor for an isotropic medium has the form Ciklm = λδik δlm + μ(δil δkm + δim δkl ), i, k, l, m = x, y, z,

(1)

ANISOTROPY OF LIQUID CRYSTALS

where λ and μ are Lamé coef cients. Any deviation of a tensor Ciklm from the form (1) corresponds to the presence of anisotropy of elasticity. In Voigt notation, the tensor Ciklm is replaced by the matrix cI J (I, J = 1, 2, . . . , 6) which, for the lowest symmetry, has 21 independent elements. The symmetry of interatomic interactions in a crystal imposes restrictions on the number of independent elements of cI J . If central forces act between atoms and every site of a crystal lattice is a center of symmetry, six Cauchy relations are satisﬁed: c12 = c66 ; c13 = c55 ; c23 = c44 ; c14 = c56 ; c25 = c46 ; c36 = c45 , which, for instance, in crystals with a heteropolar bond reduce to one relation: c12 = c44 . In hexagonal close-packed crystals no site is a center of symmetry, and the Cauchy relations do not hold even if the interatomic forces are central. The deviations from the Cauchy relations give an insight into the contribution of anharmonicity to cI J , and about nonpairwise (manyparticle) forces of interaction. Noncentrality of the interaction has a strong effect on the temperature dependence cI J = cI J (T ), as well as on the value cI I . The elements of cI J must satisfy a number of relations which are corollaries of the mechanical stability conditions for a crystal. For example, in a hexagonal close-packed crystal cI I > 0 (I = 1, . . . , 6); 2 − c2 > 0; c11 12 2 > 0; c33 (c11 + c12 ) − 2c13 2 > 0. c11 c33 − c13

Cubic crystals exhibit anisotropy of shift, which can be characterized by the factor Ashift = 2c44 / (c11 − c12 ). In addition to the shift anisotropy with the factor Ashift = c44 /c66 , crystals of hexagonal, trigonal and tetragonal symmetry have also an anisotropy of linear compressibility (with the factor Acompr = (c11 + c12 − 2c13 )/(c33 − c13 ) for hexagonal symmetry). Near the polymorphic transformation temperature, some combinations of elasticity constants can diminish abnormally (softening of normal modes). The defects in a crystal cause the components of the tensor of effective elastic moduli to decrease by several percent. When studying crystal distortions localized near defects, one needs to know elastic moduli tensors

65

of higher orders. The effective elastic moduli in a polycrystalline material are found by averaging over orientations of grains. ANISOTROPY OF g -FACTOR

A property which reﬂects the dependence of the splitting of electronic (nuclear) energy levels in a magnetic ﬁeld (see Landé g -factor) on the mutual orientation of the crystal and the ﬁeld. It manifests itself in the angular dependences of spectra of magnetic resonance, and is described by the second-rank g-factor tensor gpq (p, q = x, y, z) with unequal principal values. The magnitude of the tensor in the principal axis system for the po2 sin2 ϕ + lar angles θ, ϕ is given by g = [(gxx 2 2 2 2 2 1/2 gyy cos ϕ) sin θ + gzz cos θ] . For axial sym2 sin2 θ +g 2 cos2 θ)1/2 , where g = metry g = (g⊥ ⊥ gxx = gyy and g = gzz . Anisotropy is present in paramagnetic centers with a local symmetry lower than cubic. Ordinarily the tensor is symmetric, with gpq = gqp . ANISOTROPY OF LIQUID CRYSTALS

Dependence of physical properties of liquid crystals on the direction of a measurement.

In oriented samples the direction of the orientational order is speciﬁed by the director. If n , χ , and ε are respectively the refractive index, diamagnetic susceptibility and dielectric constant along the director, and n⊥ , χ⊥ and ε⊥ are the same quantities in a transverse direction, then

n = n − n⊥ , χa = χ − χ⊥ and εa = ε − ε⊥ are referred to as optical anisotropy, diamagnetic anisotropy and dielectric anisotropy, respectively. For example, for thermotropic liquid crystals n ∼ 0.1–0.4; χa ∼ 10−7 emu, εa ∼ 5–30. The sign of the anisotropy depends on the chemical structure of liquid crystals. For nematics (see Nematic liquid crystal), χa > 0, n > 0, εa > 0 and εa < 0. For cholesterics (see Cholesteric liquid crystal), χa > 0 and χa < 0, n < 0, εa > 0 and εa < 0. For smectics (see Smectic liquid crystal), χa > 0, n > 0, εa > 0 and εa < 0. Typical values for lyotropic liquid crystals are: χa ∼ 10−8 emu, n ∼ 10−3 . For lyotropic discotics χa > 0 and χa < 0, n > 0, for lyotropic calamitics χa > 0 and χa < 0, n < 0. Because of the anisotropy, the description of elasticity and viscosity of liquid crystals requires using several coefﬁcients.

66

ANISOTROPY OF MECHANICAL PROPERTIES

ANISOTROPY OF MECHANICAL PROPERTIES Differences in mechanical characteristics: elasticity, plasticity, and durability, along various direc-

tions of a solid. There are two types of anisotropy of mechanical properties: the natural or fundamental (primary) anisotropy, and the induced (secondary) type. The former is determined by the crystal symmetry (see Anisotropy of crystals) and can be easily observed. The latter is acquired during the process of mechanical and thermal treatment of a metal. There are two origins of secondary anisotropy: textural (see Texture) and structural. The textural type arises as a result of reorientation of crystallites along preferred crystallographic directions. The structural secondary anisotropy is caused by the oriented arrangement of grains and subgrains, inclusions of the second phase, and pores (see also Structural texture of metals). The elastic anisotropy for a number of textures can be derived analytically (see Anisotropy of elasticity). Anisotropy of plasticity and anisotropy of durability have more involved dependences than the anisotropy of elasticity, and are determined experimentally in mechanical tests. ANISOTROPY, OPTICAL See Optical anisotropy. ANNEALING Heat treatment of materials at elevated tem-

peratures aimed at investigating or improving their properties. Material annealing can lead to phase transitions, recrystallization, polygonization, homogenization, relaxation of internal stresses, removal of aftereffects of cold plastic deformation (strain hardening), annihilation and rearrangement of defects, and so on. The results of annealing depend signiﬁcantly on its kinetics: the rates of heating and cooling and the time of exposure at a given temperature. To investigate annealing of radiation-induced and other defects, use is made of isothermal annealing (long time exposure at constant temperature), and isochronal annealing (exposure during a given time interval at successively increasing temperatures). Various stages of isochronal annealing correspond to the presence of defects of different kinds. The annealing of the de-

fects of a particular type can lead to either their annihilation or their transformation into defects of more complicated types. The kinetics of isothermal annealing yield information on the nature of the reactions that result in the annealing. ANNEALING, IRRADIATION

See Irradiation annealing. ANNEALING OF SEMICONDUCTOR

See Pulsed annealing of semiconductors. ANNEALING, RECRYSTALLIZATION

See Recrystallization annealing. ANNIHILATION OF DISLOCATIONS

Merger and mutual destruction of two dislocations or elements of one dislocation loop with opposite signs (see Dislocation sign). The annihilation of dislocations leads to the disappearance (mutual compensation) of elastic e lds of dislocations. If parts of a dislocation with opposite signs come closer together as a result of dislocation slip in one common plane, then annihilation restores the perfect crystalline structure at their meeting point (see Fig. 1). The annihilation of screw dislocations occurs with the restoration of the structure even when they initially were not in the same slip plane. Nonscrew dislocations of opposite signs lying in different, but not too widely separated, slip planes form a dipole due to their mutual attraction. Its subsequent annihilation is possible by means of a head-on encounter with the creation of interstitial atoms or vacancies

Fig. 1. Annihilation of edge dislocations of opposite signs, which move in the same slip plane: (a) approach of the dislocations; (b) restoration of the perfect crystal structure upon annihilation.

ANOMALOUS DIFFUSION

67

ANOMALOUS AVERAGES

Fig. 2. Annihilation of edge dislocations of opposite signs, which move in neighboring slip planes: (a, c) approach of the dislocations; (b) formation of vacancy at the location of annihilation; (d) formation of interstitial atom at the location of annihilation.

(Fig. 2). When dislocations of opposite signs in different slip planes approach each other and reach a characteristic distance ra referred to as the annihilation radius, then the region of the crystal between them loses its stability, and annihilation occurs dynamically, rather then by diffusion. Studies of the dislocation annihilation process on an atomic scale by mathematical modeling provide the value ra ≈ (5–10)b, where b is the Burgers vector. The annihilation of dislocations plays an important role as an effective channel for reducing the dislocation density (see Dislocation density tensor) during the annealing process. This annihilation is accompanied by the emission of sound, and it is one of the most important mechanisms of acoustic emission.

The values of products of two (or more) cre+ (or annihilation akσ ) operators of halfation akσ integer spin particles (fermions), averaged over the lowest level (ground) quantum-mechanical states (at absolute zero temperature T = 0), or the thermodynamic states (at T = 0) of a system. The anomalous averages were introduced by N.N. Bogolyubov (1958) to describe superconducting (superﬂuid) Fermi systems in the self-consistent eld approximation. They provide the complex-valued order parameter (wave function) of a macroscopic coherent quantum state (see Macroscopic quantum coherence). In a superconductor at a temperature below T c , + + a−k−σ and the anomalous averages of the akσ a−k−σ akσ types are nonzero. They describe the condensate of Cooper pairs of electrons with antiparallel momenta (k = −k) and spins (σ = −σ ), which is analogous to a Bose condensate. In the super uid phases of 3 He at temperatures below 1 K (T < 0.003 K) and under a pressure (p > 30 atm), the triplet pairing of 3 He atoms with parallel spins (σ = σ ) is possible along with the singlet Cooper pairing (σ = −σ ), when the + + a−kσ and akσ a−kσ anomalous averages akσ do not vanish. In anisotropic crystals with a degenerate electron spectrum ε(k) = −ε(k + Q) and ﬂattened, nested regions of the Fermi surface separated by the wave vector Q, a spatially nonuniform state can arise. This state results from electron–hole pairing or a structural Peierls instability, and has nonzero anomalous averages of the + + ak,±σ and ak,±σ ak−Q,σ which type ak+Q,σ describe charge density waves and spin density waves.

ANODIZATION, anode oxidation

ANOMALOUS DIFFUSION A diffusion process in which the time evolution

The creation of a layer of oxide on the surface of a metal at a positive potential during electrolysis. Anodization is used to change the color, durability, hardness, electrical conductivity, catalytic activity, and other properties of surfaces of various metals and alloys. There is a great variety of electrolytes, and either direct or alternating current can be used. Depending on this, one obtains either a thin (less than 1 μm), or a thick (tens to hundreds of μm) enamel-like coating.

of the concentrations of diffusing particles fails to follow the Fick law, occurring asymptotically faster or slower than in the normal case. As for any diffusion process, anomalous diffusion is associated with a random walk of particles. However, in contrast to an ordinary random walk, the mean square displacement of a particle in the time t exhibits the behavior r 2 (t) ∼ t ν , with ν = 1. The causes of anomalous behavior are associated with the disorder of the system where the

68

ANOMALOUS DISPERSION OF LIGHT

random walk occurs. For example, anomalous diffusion behavior is observed in systems with a distribution of activation energies, when the distribution of the wait time of the next jump becomes very broad and the mean value of this time diverges; in a random walk in fractal systems the diffusion is slower (ν < 1); in a random walk with ﬂights, when a particle can travel a great distance during a short time (ν > 1), etc. To characterize anomalous diffusion, one often does not use the power index ν, but rather a related quantity called an anomalous diffusion index that characterizes properties of diffusion and random walk in a fractal system. In the normal case, for instance, on any Euclidean lattice, the square of the recession of a particle in random walk for sufﬁciently long time t is proportional to this time: L2 (t) ∼ t . In contrast to such universal behavior, the diffusion in a fractal system occurs more slowly, L2 (t) ∝ t 2/(2+θ) , where θ > 0 is the anomalous diffusion index. The quantity θ for fractal lines is related to the fractal dimension of the line D: θ = 2D − 2, although in other cases the quantity θ is some independent characteristic of a fractal system. The index θ for an inﬁnite cluster at the percolation threshold is related to well-known critical indices of percolation theory θ = (τ − β)/ν, where τ is the critical index of the percolation system conductivity, β is the critical index of the extent of the inﬁnite cluster, and ν is the critical index of the correlation length (see Correlation length). ANOMALOUS DISPERSION OF LIGHT Dispersion of light characterized by the anomalous dependence of the refractive index n of a ma-

terial on the frequency ν (wavelength λ) of the light: n decreases as ν grows (λ decreases). The anomalous dispersion of light occurs in the absorbtion bands of materials. ANOMALOUS ELASTICITY See Superelasticity. ANOMALOUS MAGNETORESISTANCE

The dependence of a conductor resistivity on the external magnetic ﬁeld, which is not describable within the classical picture of electron orbit bending (see Galvanomagnetic effects, Magnetoresistance). In magnetic materials: ferromagnetic and antiferromagnetic metals, semimagnetic

semiconductors, such departures from classic dependences (both in sign and in characteristic ﬁeld values) are related to the inﬂuence of the magnetic ﬁeld on the spin subsystem. In the case of nonmagnetic conductors, the anomalous magnetoresistance is caused by quantum-interference corrections to the conductivity, their contribution being determined by the coherence length (phase memory time) of the carriers. Such corrections arise both at weak localization (causing negative magnetoresistance), and due to interference of Coulomb and impurity scattering when the magnetoresistance is positive. ANOMALOUS MASS TRANSFER Transfer of inherent and impurity atoms in crys-

tals at a rate several orders of magnitude greater than that of diffusion. It is observed during pulse exposure causing plastic deformation with a rate greater than 1 s−1 . It results from dynamic recovery of nonequilibrium point defects formed during the process of plastic deformation under forging, explosion, pulse heating (thermoplastic deformation), in a pulsed magnetic ﬁeld (due to the action of ponderomotive forces). The mechanism of anomalous mass transfer consists in the creation of interstitial atoms under the nonconservative motion of dislocation thresholds at screw dislocations with a velocity higher than the critical one. The interaction of the moving dislocations with interstitial atoms causes the drift of the latter. Hence, the anomalous mass transfer can be treated as diffusion of nonequilibrium interstitial atoms under the conditions of drift (in the presence of driving forces of transfer processes). The distribution of the concentration C of diffusing atoms is described by the equation (x − V t)2 C(x, t) = C0 (4πDt)−1/2 exp − 4Dt x +Vt V Vx erfc √ , − C0 exp 4D D 2 Dt where C0 is the concentration at the instant of time t = 0; D is the diffusion coef cient, and V is the drift velocity in the x direction. The temperature dependence of the anomalous mass transfer rate is weaker than that of the diffusion coefﬁcient, and cannot in general be described by a simple exponential over a wide temperature range. The critical rate of deformation is deﬁned by the nonlinear

ANOMALOUS PENETRATION

dependence of the yield limit on the deformation rate. Below the critical rate, the energy of external stresses causing the dislocation slip is insufﬁcient for the formation of interstitial atoms. Therefore, only dislocation thresholds that create vacancies move conservatively. At fast rates, both vacancies and interstitial atoms are created. The latter prevail at small dislocation densities, so anomalous mass transfer diminishes with the extent of the plastic deformation. It diminishes also when an elevated concentration of excess vacancies is created in a crystal before the pulse arrival. The rise of the speed of dislocation displacement due to the swift rise of the external stresses leads to the diminishing of the vacancy contribution to the anomalous mass transfer. The dynamic multiplication of dislocations is superimposed, and the dragging along of interstitial atoms by shock waves begins to play a signiﬁcant role in the anomalous mass transfer. This transfer is faster in metals with face-centered cubic and hexagonal close-packed lattices than it is in those with a body-centered cubic lattice. The effect of anomalous mass transfer acceleration is more pronounced for substitutional impurities than for interstitial ones. As a result of the anomalous mass transfer, nonequilibrium solid solutions can also be created from the component with low mutual solubility in the solid phase. Under the low-temperature deformation of crystals with ionic bonds, other mechanisms of anomalous mass transfer appear. Thus, rather small deformation of LiF crystals at liquid helium temperatures leads to helium penetration into the surface layer of a crystal due to the dragging along of helium atoms by the dislocation thresholds, and their motion along the dislocations. Indentation (see Microhardness) of MgO crystals leads to directed plastic deformation (without the creation and motion of dislocations due to those of crowdions) (see also Anomalous diffusion). Engineering applications of anomalous mass transfer are diverse. Thus, hot forging or rolling of ingots of alloys at a deformation rate greater than the critical one allows considerable acceleration of the homogenization of dendrite liquation. Percussion welding in the solid phase forms welded joints of heterogeneous metals during a time too short for the creation of intermetallic compounds responsible for the embrittlement of the weld. The effective hardening

69

of the surface layer of machine parts is achieved by means of electric spark alloying. Taking anomalous mass transfer regularities into account leads to improving the alloyed surface layer obtained by laser processing (see Laser technology). Anomalous mass transfer occurs also at shot-blasting or ultrasonic treatment of a metallic coating on the surface of products. The mechanical mixing of surface layers of contacting metals under shock loading known as mechanical diffusion does not fall into the category of anomalous mass transfer. ANOMALOUS PASSAGE OF X-RAYS, Borrmann effect (G. Borrmann, 1941) Propagation of X-rays in monocrystals along directions satisfying the Bragg law, when the ef-

fective (so-called interference) absorption coefﬁcient is considerably smaller than the photoelectric absorption coefﬁcient μ. This is observed in the case of Laue diffraction for sufﬁciently thick crystals at absorption levels μt 3–5 (t is the sample thickness). The anomalous passage of X-rays is the result of multiple scattering by atomic planes of a crystal, and the interference of the scattered waves, which leads to the creation of a total wave ﬁeld with a spatially modulated amplitude. If the antinodes of this ﬁeld lie to the side of atomic planes, it is absorbed very weakly (much more weakly than in ordinary interference). As a result, the X-rays can travel in crystals for relatively great distances (up to 1–10 mm). The anomalous passage was ﬁrst observed in perfect crystals; and has subsequently been seen in mildly distorted crystals. It occurs for the diffuse background as well, which leads to considerable, often asymmetric deformation of the diffuse scattering of X-rays proﬁle compared to the kinematic case (ampliﬁcation of central part of the proﬁle relative to its wings). See also Dynamic radiation scattering, Two-wave approximation. ANOMALOUS PENETRATION of the electromagnetic eld into a metal

This occurs in an external magnetic ﬁeld, and is caused by the speciﬁc dynamics of the conduction electrons. The effects of anomalous penetration are subdivided into two groups. The ﬁrst group, that of plasma or collective phenomena, comprises the aggregate of weakly decaying waves in the degenerate electron plasma of a metal (see Helicon,

70

ANOMALOUS PENETRATION OF ULTRASOUND

Magnetic plasma waves, Cyclotron waves, Quantum waves, Doppleron, etc.). The second group in-

cludes ballistic effects of anomalous penetration which are caused by a trajectory transfer of an electromagnetic wave from the skin depth layer δ into the bulk metal by numerous groups of electrons, involving individual motions of the charged particles and quasi-particles. Because of the skineffect, the most effective interaction of the electrons with the electromagnetic ﬁeld occurs for those electrons which move along the wavefront, i.e. parallel to the surface of the metal (so-called effective electrons). Electrons moving at large angles with the surface spend less time in the skin layer, and thus are less effective in gaining energy from the wave. In a magnetic ﬁeld the direction of the electon velocity changes periodically due to the cyclotron motion. Therefore, the most intense interaction with the electromagnetic wave occurs in the vicinity of points of electron trajectories where the velocity is parallel to the surface (so-called effective points). Due to the cyclotron motion the number of these points is inﬁnite, and under the anomalous skin-effect δ D (D is the characteristic length of a trajectory), some of these points are located outside the skin layer. Their existence is related to resonant excitation of the electron collective motion. When moving inside this layer the electron acquires a velocity increase

v and creates the current j = −e v, where e is the magnitude of the electronic charge. At the next effective point lying in the depth of a metal, the electron again moves parallel to the sample surface and reproduces the current increment j there. This is what constitutes anomalous penetration of the ballistic type: bursts of current and magnetic ﬁeld spaced by the distance D arise inside the metal. The various types of electron trajectories lead to different mechanisms of anomalous penetration. In a magnetic ﬁeld B parallel to a metal surface, due to the complicated structure of the Fermi surface, there exists anomalous penetration along the chain of (closed) electron trajectories with extremal diameters Dext (see de Haas–van Alphen effect). The chain of trajectories from the central section of the Fermi surface is created in a slightly tilted B. At a greater inclination of B there occurs a kind of focusing of effective electrons drifting into the interior of the metal. These electrons

provide bursts of anomalous penetration at depths that are multiples of the displacement along the normal to the sample surface, extremal over the cyclotron period. This mechanism of anomalous penetration is related to a sharp rise of the Fourier component of the conductivity due to Dopplershifted cyclotron resonance. The following effects arise from the drift type of anomalous penetration: focusing of electrons from the vicinity of the reference point of the Fermi surface, bursts on the helical paths of the Fermi surface boundary cross sections, trajectory transfer by effective electrons on an open Fermi surface, etc. Finally, in a magnetic ﬁeld perpendicular to the metal surface, the ballistic effects of anomalous penetration are associated with the magnetic focusing of drifting or ineffective, electrons, the so called Gantmakher– Kaner effect. The various phenomena of anomalous penetration of trajectories of weakly damped waves are closely interrelated, and can transform into each other when the frequency ω or the magnetic ﬁeld B is changed. The physical pattern of anomalous penetration depends on the nature of the reﬂection of electrons from the metal surface. The anomalous penetration of radio waves manifests itself experimentally as a radio-frequency size effect. It is used to investigate Fermi surface parameters, the temperature dependence and anisotropy of the mean free path, and mechanisms of surface electron scattering. ANOMALOUS PENETRATION OF ULTRASOUND into a metal

A signiﬁcant nonlocal phenomenon appearing at high frequencies ω, when the damping depth of a sound wave (calculated within the framework of a local theory), L ∼ = vF /ω, is smaller than the mean free path of the carriers, l = vF τ (the latter is the penetration depth of electron density oscillations caused by sound, and interacting with it in a conductor; see Anomalous skin-effect). Thus, the anomaly criterion is ωτ 1 for the asymptote of the acoustic ﬁeld u(x, t) in the bulk of a metal (x L), when it is a relatively weak but slowly damped quasi-wave (non-exponentially damped in the collision-free limit) propagating with the electron velocity vF . The appearance of electron-acoustic quasiwaves is associated with the degenerate statistics

ANOMALOUS PHOTOVOLTAIC EFFECT

of charge carriers in metals, i.e. with the presence in the electron spectrum of a Fermi velocity in every direction. Anomalous penetration of ultrasound occurs for an arbitrary electron dispersion law, and for any polarization of the sound. In the typical case of a convex Fermi surface and monochromatic longitudinal vibrations, we have ωx s2 u(x, t) ∼ ln−2 = Cu(0, t) vF0 ωx vF0 x iωx , − × exp vF0 l0 vF0 x . ω Here C is a numerical factor of the order of unity determined by the form of the electron spectrum, and the nature of their reﬂection from the metal boundary (x = 0); s is the sound velocity, and vF0 = (vx )max is the electron velocity at the reference point on the Fermi surface. The quasi-waves are generated also by other particular values of vx on the Fermi surface; the power law of asymptotic decay u(x) ∼ x −3/2 as l → ∞ is characteristic for an internal extremum of vx on a nonconvex Fermi surface. With respect to short (compared with τ ) acoustic pulses, the anomalous penetration of ultrasound is revealed in the formation of an acoustic signal “forerunner” by electrons. In the absence of a magnetic eld the quasi-wave precursor travels with the velocity vF0 . Hence, the observation of the anomalous penetration of ultrasound in the pulse mode could make it possible, by varying the geometry and width of samples, to measure directly both electron velocities and local values of their mean free paths over the entire Fermi surface of the metal under study. Observed in the magnetic ﬁeld B in the pulse mode is the ultrasound ﬁeld transfer by conduction electrons along the electron orbit chain (the analogue of bursts of the electromagnetic ﬁeld). Having effectively interacted with the ultrasonic ﬁeld in the region where vx = s, the fast electron carries away the information on the sound pulse to create its “image” at its path locations where vx = s again. As a result, the forerunners and afterrunners of the sound signal arise, the distance between them (in the absence of electron drift along x) being a multiple of the extremal diameter of an electron orbit. To identify the effect

71

unambiguously, the generating ultrasound pulse width must be much less than the Larmor diameter. Otherwise, the effect appears as oscillations of the sound speed as the magnetic ﬁeld changes. The shape of the forerunners repeats that of the generating pulse. The analogue of the anomalous penetration of ultrasound is the anomalous penetration of an alternating longitudinal (i.e. normal to the interface) electric ﬁeld. Though its main part decays exponentially into the metal for a distance that approximates a Debye radius, the nonuniformity of the electron density remains down to macroscopic depths ∼ = l. Owing to the deformation interaction of a nonequilibrium electron gas with the ionic lattice vibrations, this leads to a new (linear in the applied ﬁeld amplitude) mechanism of electronacoustic transformation, where efﬁciency grows as ωτ increases. Such an effect related to the anomalous penetration of ultrasound was ﬁrst observed in a tin single crystal at liquid helium temperatures. ANOMALOUS PHOTOCONDUCTIVITY Photoconductivity which is characterized by

unusual behavior, such as: independence of the photocurrent from the photoexcitation intensity over a wide range, marked dependence on the spectral content of the light, and long-term relaxation of the photoconductivity after extinction of the light. Anomalous photoconductivity was discovered and investigated in detail on layers of amorphous selenium treated in mercury vapors. It is explained by the existence of deep traps for mobile particles with small probabilities of both thermal excitation of electrons to the conduction band, and recombination with a free hole. The traps are assumed to be clusters containing about 103 atoms, and localized in a region near the surface of the sample. Anomalous photoconductivity is sometimes referred to as the phenomenon of current reduction under illumination, but in this case the term negative photoconductivity is more often used. ANOMALOUS PHOTOVOLTAIC EFFECT

Appearance of a voltage Vp during illumination of a sample by light of energy in excess of the band gap Eg .

72

ANOMALOUS SKIN-EFFECT

Under ordinary mechanisms of the photoelectromotive force: eVp Eg (see Photoelectric phenomena). Anomalous photovoltages are observed in semiconductor ﬁlms (e.g., CdTe), in lithium niobate crystals, selenites and other materials exhibiting unipolarity along some direction. The values of Vp in the anomalous photovoltaic effect can be as high as many kilovolts. This effect can occur either with the absence of a center of symmetry of the crystal lattice, or with a certain nonuniformity of the distribution of defects in the sample. In the ﬁrst case, the appearance of a photovoltage provides for the transfer of free current carriers in one of the directions along the unipolar axis during the process of photoexcitation (such a mechanism was discovered experimentally in lithium niobate crystals), or is responsible for the unipolar character of current carrier scattering by oriented dipoles created by lattice defects. In the second case, the cause of the anomalous photovoltaic effect can be the formation of interconnected microscopic sources of electromotive forces, e.g., semiconductor junctions. This mechanism has been used to explain the anomalous photovoltaic effect in semiconductor ﬁlms. ANOMALOUS SKIN-EFFECT

A variety of phenomena of electromagnetic ﬁeld damping in metals (and plasma) under the condition that the mean free path l of conduction electrons considerably exceeds the skin layer depth, δ. In contrast to the normal (classical) skineffect when l δ and electromagnetic absorption is determined by collisions of conduction electrons with scatterers, the mechanism of absorption in the anomalous skin-effect has the collisionfree character of Landau damping. The screening of the external wave by the conductor in this effect is caused by the sliding (so-called effective) electrons that move almost in parallel to the surface at angles on the order of δ/ l. The salient features of the anomalous skin-effect are the non-exponential decay of the amplitude of an electromagnetic wave deep inside the metal, independence of the skin layer depth δ on l (in the normal skin effect δ ∝ l −1/2 ), a different frequency dependence of the surface impedance Za ∝ ω2/3 (whereas Zn ∝ ω1/2 ) and the change of the relation between its real and imaginary parts. The

value of the impedance in the anomalous skineffect depends on the character of electron scattering at the surface: under diffuse reﬂection, and the impedance is 12.5% greater than under specular reﬂection. The anomalous skin-effect has been observed in pure monocrystals of metals at low (helium) temperatures in the frequency range from several to hundreds of GHz. It was discovered by H. London (1940) in tin. ANOMALOUS THERMAL EXPANSION

Excessive thermal expansion of the lattice surface (in the ﬁrst 1–2 monolayers), which takes place in semiconductors, metals and simple chemical compounds. For example, the ratio of the linear thermal expansion coefﬁcient (normal and tangential) of the surface to its bulk value for a Si crystal is approximately 8, for Ge: 4, for GaAs: 3, for NaF and LiF: 2, for W: 2–3. Anomalous thermal expansion was established by various methods: low-energy electron diffraction, scattering of H and D atoms, spin polarization of reﬂected lowenergy electrons. This expansion does not harm the crystal surface (for moderately high temperatures) due to the relaxation (compression) of the surface layers of the lattice, and the presence of monatomic steps and other defects on the crystal surface. For instance, under heating to 500 K the lattice parameter of bulk LiF will rise by 1.5%, while the increase on the surface is 3%. The extra expansion (1.5%) of the surface is compensated by surface relaxation or structural defects. ANOMALY, KOHN See Kohn anomaly. ANTHRACENE, C14 H10 (fr. Gr. ανϑρας , coal)

An aromatic conjugated, condensed three ring hydrocarbon with molecular weight 178.22. A crystal of anthracene (speciﬁc weight 1.25 g/cm3 ; T melting = 217.8 ◦ C; T boiling = 355 ◦ C) consists of anthracene molecules bonded by weak van der Waals forces; it is a typical representative of molecular crystals. Crystals of anthracene belong to the prismatic monoclinic sys5 ) and two moletem with space group P 21 /c (C2h cules per unit cell. The monoclinic axis b, the

ANTIFERROELECTRICITY

crystal symmetry axis, coincides with the middle axis of the refractive index ellipsoid. Crystals of anthracene can be produced by sublimation, as well as by crystallization from the melt (Bridgeman’s method), or from solution. Using monocrystal growth by sublimation one obtains thin (from a fraction to hundreds of microns) colorless foils, their blue uorescence being readily observable under ordinary illumination (quantum yield of ﬂuorescence close to unity). The plane of these foils contains the a and b axes of the crystal. Anthracene is easily soluble in hot benzene, poorly soluble in alcohol, ether, and is insoluble in water. It is crystallized from solution to form colorless prisms. Using the Bridgeman method, one can obtain large crystals with any developed plane. Crystals of anthracene begin to absorb light in the near ultraviolet region. The Davydov splitting of the 0–0 band of the ﬁrst electron transition is equal to 230 cm−1 . Under irradiation with ultraviolet light anthracene can be dimerized or oxidized to anthraquinone. A crystal of anthracene is an organic semiconductor, and it is the basis of several large groups of dyes. Many valuable natural substances are anthracene derivatives (alizarin, cochineal, chrysophanic acid, etc.). Anthracene lm s produced by spraying can be used as nonsilver carriers for information recording. ANTICORROSIVE COATINGS

Layers of material applied to metal parts for corrosion protection.

The protection is assured either by insulation of the construction metal from the corrosive environment, or due to the protective or inhibitory action of the coating upon the metal being protected. In terms of composition, anticorrosive coatings are classiﬁed into nonmetallic, metallic and composite; and in terms of their mode of action they can be insulating, protecting and inhibiting. Concerning their durability, coatings are protective (for a given service life) and preserving (temporary protection). Some important properties of the coatings are their chemical resistance, porosity (permeability), adhesion to the basic metal, and deformability. The tin, lead, copper, nickel, chrome, and titanium coatings are classiﬁed as corrosion resistive (insulating) metallic coatings, while zinc, cadmium, aluminum coatings on steel are protective types.

73

Concerning their mode of application metallic coatings are subdivided into electroplated, hotdip (of the melted metal) and metallized ones. The nomenclature of metallized coatings is quite diverse, and is differentiated by the deposition method (electric arc, gas-ﬂame, plasma, and gasthermal metallization). To create coatings or corrosion layers on the metal surface, one can also use electrolysis from melted salts, deposition from gas-vapor phase, and implantation of metal ions or noble gases. To improve the operating protective properties of the surface layer, use is often made of diffusive heating that provides for diffusion of coating components into the underlying metal. The greatest scope of application (about 70%) involves protective polymeric (and ﬁlm) lacquer paint coatings, protective fettle coatings, protective enamel and other inorganic nonmetallic coatings differing in their chemical composition, technology of application and range of use. Composite metal-polymer coatings, inhibited metallic and nonmetallic coatings that provide better reliability and protection duration have gained wide use as well. ANTIEMISSION MATERIALS Metals, alloys, chemical compounds exhibiting

low intensity of electron emission or its absence. The antiemission materials include gold, platinum, titanium, zirconium, carbon, carbides of tungsten and molybdenum, titanium silicides, and others. They are used for coating the working surfaces of instruments, as well as their nonoperational surfaces to suppress electron emission during their useful lifetime. ANTIFERROELECTRICITY (fr. Gr. αντ ι, against, and ferroelectricity)

A set of phenomena related to the appearance of ordered antiparallel electric dipole moments in the crystal lattice of antiferroelectric crystals. The spontaneous polarizations (see Ferroelectricity) of neighboring ionic chains or dipole groups of the same type are oriented in opposite directions, so the total polarization is zero. Phases having the free energy (see Thermodynamic potentials) close to that of pyroelectric and ferroelectric states are usually considered favorable for forming antiferroelectric phases, because the phase transitions to paraelectric and ferroelectric states are

74

ANTIFERROELECTRICS

possible from these phases under a change of temperature, application of electric ﬁeld, pressure, and substitutions for some lattice ions. The electric ﬁeld decreases the temperature of an antiferroelectric phase transition and increases the dielectric constant ε. There are antiferroelectric phases with their structure change explainable by condensation of several soft modes having wave vectors on the Brillouin zone boundary. The phase transition from the para- to the antiferromagnetic phase is accompanied by a change in the lattice superstructure, reduction of ε, spontaneous strain, changing the birefringence and quadrupole bond constant, elastic and electrooptical properties, etc. More than 60 antiferroelectric compounds are known with many different structures. Some of them have a displacive type phase transition (e.g., PbZrO3 , NaNbO3 , PbMg1/2 W1/2 O3 ), and others with the perovskite type structure undergo an order–disorder phase transition (also NH4 H2 PO4 , Cu(HCOO)2 ·4H2 O). There are incommensurate nonpolar phases which are antiferroelectric in the crystals NaNO2 , Rb2 ZnCl4 and others. Antiferroelectrics are used as electrooptic materials and as components of various solid solutions, which are the bases of capacitor, piezoelectric materials and electrostriction materials for optics, electronics, radio engineering, and so on. ANTIFERROELECTRICS Insulators with internal oppositely directed elec-

tric dipole moments due, for example, to rows of ions displaced in opposite senses. A transition from the high-temperature paraelectric phase to the low-temperature ordered, antiferroelectric state occurs via a structural phase transition, which is accompanied by a considerable anomaly in the dielectric constant. The transition temperature TC typically depends strongly on the applied electric ﬁeld, so antiferroelectricity can be induced by the application of a ﬁeld, as well as by lowering the temperature. Since the transition is typically a r storder phase transition, a jump-like change in the polarization P is observed as the ﬁeld E changes, and the dependence P (E) has the shape of a (possibly double) hysteresis loop (see Hysteresis). Typical antiferroelectrics are NH4 H2 PO4 (TC = 148 K), PbZrO3 (TC = 506 K), and NaNbO3 (TC = 627 K).

ANTIFERROMAGNET

A material with antiferromagnetic ordering of magnetic moments of atoms and ions (see Antiferromagnetism).

A substance becomes antiferromagnetic when cooled below its Néel point T N , and generally remains in this state down to T = 0 K. Elemental antiferromagnets are: solid oxygen (α-modiﬁcation) at T < 24 K; Mn (α-modiﬁcation) with T N = 100 K; Cr (T N = 310 K); a number of rareearth metals (with T N from 12.5 K for Ce to 230 K for Tb). Chromium has a sinusoidally modulated magnetic structure, and the heavy rare-earth metals also have complicated magnetic structures provided by neutron diffraction (see Magnetic neutron diffractometry). In the temperature range between T1 and T N (0 < T1 < T N ), they are antiferromagnetic, and below T1 they become ferromagnetic. Chlorides of Fe, Co and Ni were the ﬁrst known antiferromagnets, and by now thousands of them are known. The chemical formula includes at least one transition ion. Antiferromagnets include numerous simple and complex oxides of transition elements such as ferrite spinels, iron garnets, orthoferrites and orthochromites, as well as ﬂuorides, sulfates, carbonates, etc. There are a few antiferromagnetic organic compounds, as well as metallic alloys, in particular alloys of the iron and platinum groups. The temperature dependence of the speci c heat has a maximum at T N which is typical of a second-order phase transition. Noted among cubic antiferromagnets is the family of rare-earth ferrite garnets in which Fe is replaced by Al or Ga. Dysprosium-aluminum garnet Dy3 Al5 O12 is of special interest because it is an antiferromagnetic Ising magnet in which the anomalous behavior close to the triple critical point has been studied in detail. The detailed investigation of hydrous copper chloride (CuCl2 ·2H2 O) led to the discovery of antiferromagnetic resonance, magnetic phase transition – reversal of sublattices (spin-ﬂop transition) in a magnetic ﬁeld, and weak antiferromagnetism. Noted among uniaxial crystals with anisotropy of the easy-axis type is the group of ﬂuorides (MnF2 and others), which served to clarify optical absorption spectra and provided the discovery of exciton-magnetic excitations, two-magnon absorption, and Raman scattering of light by

ANTIFERROMAGNETIC DOMAIN

magnons. The optical absorption spectra were also investigated with binary ﬂuorides like KMnF3 , CsMnF3 . Brillouin scattering of light by magnons was observed in antiferromagnetic FeBO3 and CoCO3 . In uniaxial CoF2 the piezomagnetic effect was discovered (see Piezomagnetism), and in Cr2 O3 the magnetoelectric effect. In uniaxial crystals with anisotropy of the easy-plane type (α-Fe2 O3 , MnCO3 , CoCO3 , NiF2 ) the weak ferromagnetism due to the Dzialoshinskii interaction was discovered. Of special interest among substances with weak ferromagnetism are the orthoferrites (YFeO3 and others) where orientational phase transitions (the change of the antiferromagnetic ordering axis) are observed, and transparent FeBO3 with T N above room temperature which displays a magnetoelastic interaction. The strongest magnetoelastic interaction among antiferromagnets is observed in α-Fe2 O3 . This is the ﬁrst compound to exhibit a wide gap in the spin wave spectrum that equals E = γ (2B ME B E )1/2 and is caused by the effective ﬁeld of magnetoelastic anisotropy B ME (B E is the exchange ﬁeld) (see Magnetoacoustic resonance). Some antiferromagnets contain more than two magnetic sublattices. For example, uranium oxide (UO2 ) is a four-sublattice antiferromagnet characterized by three antiferromagnetism vectors that form an orthogonal vector triplet. There is a group of antiferromagnetic semiconductors (chalcogenides of Mn, Eu, Gd and Cr) with very strong magnetooptical effects. The low-dimensional antiferromagnets are of particular theoretical interest. The already mentioned Fe and Co ﬂuorides as well as some binary ﬂuorides BaCoF4 , Rb2 CoF4 are two-dimensional antiferromagnets. The well-known metal-oxide compounds displaying properties of high-temperature superconductivity (La2 CuO4 , YBa2 Cu3 O7−δ ) in their insulating phase are many-sublatticed quasi-two-dimensional antiferromagnets. Onedimensional antiferromagnets include KCuF3 , CuCl2 , RbNiCl3 and others. Especially strong interactions of electron and nuclear spin system oscillations were observed in KMnF3 , MnCO3 , and CsMnF3 . Anhydrous sulfates of copper and cobalt as well as CoF2 exhibit antiferromagnetic ordering induced by a magnetic ﬁeld at temperatures above T N due to the Dzialoshinskii interaction.

75

The values of T N of most antiferromagnets lie below room temperature. ANTIFERROMAGNETIC DOMAIN A region of an antiferromagnet with a constant value of the antiferromagnetism vector L =

M 1 − M 2 . The directions of L in different antiferromagnetic domains are different. Antiferromagnetic domains are separated by antiferromagnetic domain walls. It is not always true that the division of antiferromagnets into domains results in a decrease of the energy of the demagnetization elds. The appearance of these domains either in the intermediate state of magnets, or for antiferromagnets with a weak ferromagnetism, is thermodynamically favorable. In other cases, these are thermodynamically unfavorable. In addition in some cases, e.g., for domains with zero magnetization and differing in the sign of L (antiferromagnetic domains with 180◦ neighbors), states in different domains, within the macroscopic framework, are considered identical because they differ from one another only in the redesignation of the magnetic sublattices. This is a substantial distinction of the properties of antiferromagnetic domains in comparison to, e.g., those of ferromagnets with different directions of magnetization. The presence of antiferromagnetic domains in real antiferromagnets can be linked with the fact that a magnetic phase transition to an antiferromagnetic state due to nonuniformity can occur independently in various ﬁnite regions of a crystal. If these regions differ in the sign of L, then the spreading of the transition over the whole sample causes antiferromagnetic domains to appear. In addition, the division of antiferromagnets into domains can reduce the energy of elastic strain, or (at moderate temperatures, near the Néel point) become thermodynamically favorable due to the contribution of entropy to the free energy of the antiferromagnet. These domains signiﬁcantly affect such properties as the electrical conductivity of a metal antiferromagnet, and sound absorption in some antiferromagnets. The presence of antiferromagnetism hinders the observation of a series of effects sensitive to the sign of L, e.g., piezomagnetism. Antiferromagnetic domains of the non180◦ kind (so-called T-domains or twin domains) are accompanied by a distortion of the crystal lattice, thus providing a way to detect, for example, a

76

ANTIFERROMAGNETIC METALS

conversion of an antiferromagnet to a single domain state, and to study it by various methods. The observation of the 180◦ antiferromagnetic domains (S-domains, i.e. spin-rotation domains) was carried out by using the linear magneto-optic effect. Those domains, in which this effect is allowed by the symmetry in the external magnetic ﬁeld, possess optical properties dependent on the direction of L, which allows one to employ optical methods for magnetic domain characterization. ANTIFERROMAGNETIC METALS Solids with metallic conductivity exhibiting antiferromagnetism. They include a number of 3d-, 4f -, and 5f -metals, their alloys and some

of their compounds. When analyzing the physical mechanism responsible for antiferromagnetism in the metals, it is important to know to what extent the electrons responsible for the magnetic ordering (magnetic electrons) are localized. Accordingly, one can speak about band antiferromagnetism (see Band magnetism) and the antiferromagnetism of magnetic ions. In band antiferromagnets the magnetic electrons form a relatively wide, partially ﬁlled band with the exchange splitting ε ζ , where ζ is the chemical potential referenced to the bottom of a band. These materials are described in terms of a static spin density wave with a wave vector k that can be either commensurate or incommensurate with a reciprocal lattice period (see Incommensurate structures, Modulated magnetic structures). A strict theory exists solely for the case of weak band antiferromagnetism ( ε ζ ). An example is pure Cr with the Néel point T N = 312 K. Below this temperature, the magnetic moment per atom is μ = 0.59μB (μB is Bohr magneton), much less than that of an isolated Cr atom (μ = 3μB ). The spin density wave period is incommensurate with the reciprocal lattice period k = (2π/a)(1 − δ, 0, 0), where a is the lattice constant. At T = 118 K, δ = 0.049 and depends slightly on the temperature; at T = T N , δ = 0.037. Chromium alloys can exhibit both commensurate and incommensurate spin density waves, the origin of latter being determined by the speciﬁc nature of the Fermi surface, which includes congruent hole and electron octahedra whose component parts can be made coincident with themselves via

translation by a reciprocal lattice vector k. It is the triplet pairing of electrons (holes) of congruent parts that manifests itself as a spin density wave with wave vector k. The presence of congruent parts of Fermi surfaces leads to instability of the paramagnetic state with respect to the emergence of a spin density wave (spin density wave instability). Weak band antiferromagnets include compounds with metallic conduction CrB2 (T N = 85 K), VX, VX2 , V3 X4 , V5 X8 , where X ≡ S or Se (for VS T N = 1040 K, for V3 S4 T N = 9 K, for V3 Se4 T N = 16 K, for V5 S8 T N = 29 K, for V5 Se8 T N = 35 K). The weak band antiferromagnet MnSi possesses a helical structure (see Helicomagnet) with a long wavelength (180 Å) and hence it may be considered as a weak band antiferromagnet with an inhomogeneous ground state in the form of a helical spin density wave. The examples of strong band antiferromagnets are: α-Mn (T N = 95 K); γ -Mn (T N = 450 K), γ -Mn being metastable in the region of antiferromagnetism (it is stable only at T > 1352 K); γ -Fe (T N = 8 K; γ -Fe is stable in the range 910–1400 ◦ C). They all support commensurate spin density waves. Antiferromagnetism of magnetic ions takes place in rare-earth metals due to the smallness of the radius of 4f -shells whose electrons are responsible for the magnetic ordering (see Magnetism of rare-earth metals). Rare-earth metals are commonly classiﬁed into light (from Ce to Eu) and heavy (from Gd to Lu) ones. The light rare-earth metals (except Nd) at T N are antiferromagnets with a collinear structure. In the heavy rare-earth metals (except Gd, Yb, Lu) and in Nd, an antiferromagnet–ferromagnet transition is observed at a lower temperature T = T c < T N in addition to the paramagnet–antiferromagnet transition at T = T N . In the antiferromagnetic range T N –T c , magnetic moments of rare-earth metals create complicated modulated magnetic structures (helical, cycloidal, sinusoidal). The complicated magnetic structures arise also in alloys of rareearth metals with each other and with Y (a paramagnet in the pure state). The Néel temperatures of the light rare-earth metals are as follows: for Ce T N = 12.5 K; for Pr T N = 20 K; for Sm T N = 14.8 K; for Eu T N = 90 K; for Nd T N = 19 K with ferromagnetism observed below T c = 7.5 K.

ANTIFERROMAGNETISM

Intermediate type of antiferromagnetic metals. The magnetic order of a number of antiferromagnetic metals is determined by the presence of two factors: spin density wave instability (near congruent parts of Fermi surface) and localized magnetic moments (FeRh, Pt3 Fe, alloys: Cr–(Fe, rare-earth metal), Mn–rare-earth metal, Y doped with rareearth metal). Small additions of rare-earth metals to paramagnetic Y cause a helical antiferromagnetic structure to appear. In compounds FeRh, Pt3 Fe, one part of the Fermi surface exhibits spin density wave instability, while another forms local moments. Antiferromagnetic actinides: pure metallic curium (T N = 52 K) and several compounds with metallic conductivity: UP (130 K), UAs (182 K), USb (213 K), UBi (290 K) (T N given in parentheses). ANTIFERROMAGNETIC RESONANCE

The selective absorption by an antiferromagnet of electromagnetic wave energy with a frequency close to the natural frequencies of precession of magnetization vectors of magnetic sublattices; a variety of electron magnetic resonance. Antiferromagnetic resonance involves the excition of resonant coupled oscillations of magnetization vectors of magnetic sublattices of the antiferromagnet relative both to each other and to the direction of the applied magnetic ﬁeld B 0 (see Antiferromagnetism). The frequency of these oscillations is determined by the value of effective magnetic ﬁelds acting on magnetic moments of sublattices: B E , the effective ﬁeld of the exchange interaction of sublattices, B A the ﬁeld of magnetic anisotropy, and B 0 . The dependence of the resonance frequency ω on the effective magnetic ﬁeld in antiferromagnets is complicated, and depends on the crystal structure. When the external magnetic ﬁeld is applied parallel to the easy magnetization axis then two antiferromagnetic resonance frequencies lying in the range 10–100 GHz correspond to one value of B 0 . The study of antiferromagnetic resonance makes it possible to determine the value of effective magnetic ﬁelds in antiferromagnets.

77

ANTIFERROMAGNETISM

Magnetically ordered state of a crystalline material in which neighboring atomic magnetic moments are aligned antiparallel, and the total magnetic moment of a magnetic unit cell of the crystal equals zero (or a very small fraction of an atomic moment). Antiferromagnetism occurs at temperatures below the Néel point T N . More generally, antiferromagnetism refers to the set of physical properties associated with the antiferromagnetic state. The exchange interaction seeking to align the spins and hence the magnetic moments antiparallel to each other is responsible for the antiferromagnetism. The idea that the exchange interaction can cause antiferromagnetism was put forward by L. Néel (1932) and independently by L. Landau (1933), who, in addition, described theoretically the phase transition from the paramagnetic to the antiferromagnetic states. At T > T N , when the thermal energy (E = k B T ) exceeds the exchange energy (μB E , where μ is the atomic magnetic moment and B E is the exchange ﬁeld), the material exhibits paramagnetic behavior (see Paramagnetism). The temperature dependence of the magnetic susceptibility χ of such a material at T > T N follows the Curie–Weiss law χ = C/(T − θ) with a negative Weiss constant θ , and C is a constant. At T = T N , antiferromagnetism appears in a material. In most cases the phase transition at T N is a secondorder transition accompanied by the characteristic anomalies of magnetic susceptibility, speci c heat, thermal expansion coefﬁcient, elastic moduli, etc. The magnetic ordering is characteristic of an atomic magnetic structure with a symmetry described by point and space magnetic symmetry groups. The magnetic structure of an antiferromagnet is conveniently described by two, four, or more interpenetrating magnetic sublattices with magnetizations M j that mutually compensate each other. As an example, Fig. 1 shows two antiferromagnetic structures: (a) MO, where M = Mn2+ , Ni2+ , Fe2+ ; (b) MF2 , where M = Mn2+ , Co2+ , Fe2+ . The difference is that the ﬁrst one has a cubic magnetic unit cell with lattice parameter a M twice that of the crystallographic unit cell (a C ), while the magnetic unit cell in the second (tetragonal) structure coincides with the crystallographic

78

ANTIFERROMAGNETISM

Fig. 1. Magnetic structure the antiferromagnets (a) MnO and (b) MnF2 .

one. In most antiferromagnetic materials with

no external magnetic ﬁeld present, M i = 0. However, there exists a large group of antiferromagnetic materials for which this condition is not strictly met. They are materials with weak ferromagnetism (weak ferromagnets), in which M i |M i |. There are also more complicated antiferromagnetic structures, which can not be described in terms of sublattices. They are helical and sinusoidal antiferromagnets (see Modulated magnetic structures, Spin density wave). In both types a preferred direction exists. In the helical structure, the spins of all magnetic atoms in each crystallographic layer perpendicular to the preferred direction are parallel to each other. However, the direction of magnetization of each layer is turned relative to the neighboring ones by some angle ϕ = π/n, where n is typically a noninteger number. In sinusoidal structures, the magnetizations of layers are not parallel to each other, but their value varies according to the law Mk = M0 sin(k ϕ). Both structures are incom-

mensurate in the sense that the magnetic and crystallochemical translational periods are not multiples of each other. In most antiferromagnetic materials, the directions of magnetization vectors M i relative to crystallographic axes are determined by much weaker interactions than the exchange (E ex ) interactions, causing the anisotropy of antiferromagnetic materials (E a ) (see Magnetic anisotropy). The axis along which the magnetizations of sublattices are aligned is known as the easy axis. Antiferromagnetic materials with E a E ex , referred to as metamagnetics, do not exhibit a spin-ﬂop transition (see Magnetic phase transitions). Also referred to as metamagnetics are layered antiferromagnets in which the exchange interaction E ex inside a layer is ferromagnetic and much stronger than the antiferromagnetic interaction between the layers. A direct method to determine the antiferromagnetic structure (including the direction and even the temperature dependences of the sublattice magnetizations) is magnetic neutron diffractometry. The intensity of magnetic diffraction peaks is proportional to the square of the sublattices magnetization. In real antiferromagnetic substances antiferromagnetic domains exist. In weak magnetic ﬁelds, the magnetization M in antiferromagnetic materials, as well as that in a paramagnet, depends linearly on the magnetic ﬁeld (M = χB); however, the temperature dependences of χ in these substances differ signiﬁcantly. In uniaxial crystals the salient features of antiferromagnetism (e.g., anisotropy of magnetic susceptibility) are exhibited most clearly. In particular, the longitudinal (along the antiferromagnetism axis) magnetic susceptibility χ decreases sharply as temperature T decreases, while the transverse one χ⊥ is almost independent of the temperature (Fig. 2). Thus, there is a strong anisotropy of the magnetic susceptibility. If the magnetic ﬁeld directed along the easy axis attains the critical value B c1 = (2B A B E )1/2 (B A is the effective anisotropy ﬁeld), magnetic sublattices ﬂip over in the direction perpendicular to the magnetic ﬁeld. This spin-ﬂop transition occurs because at B > B c1 the difference of magnetic energies in the easy axis and ﬂipped over states becomes greater than the anisotropy energy E A : (1/2)(χ⊥ − χ )B 2 /μ > E A . In samples of ﬁnite

ANTIFERROMAGNETISM

79

Fig. 2. Anisotropy of the magnetic susceptibility χ in an axial antiferromagnet. Fig. 3. Spectrum of spin waves in MnF2 .

size, the intermediate state with alternating layers of ﬂipped over and normal phases is formed in the narrow region of ﬁelds near B c1 due to the energy of demagnetization. There exists a second critical ﬁeld B c2 = 2B E at which the antiferromagnetism is destroyed completely, and all magnetic moments align strictly parallel to the applied ﬁeld (i.e. a spin-ﬂip transition occurs). Other magnetic phase transitions are observed in antiferromagnets as well. A theoretical description of antiferromagnetism can be given within both phenomenological and microscopic models. A phenomenological description based on the Landau theory of secondorder phase transitions uses the expansion of the free energy in even powers of components of magnetization vectors of magnetic sublattices, taking into account the crystal symmetry. This theory predicts symmetries of magnetic phases, as well as the shape of phase diagrams in the vicinity of TN . The microscopic theory uses a Heisenberg Hamiltonian written in terms of spin operators, and leads to the energy of the “ground” state and a spectrum of spin waves. In contrast to ferromagnets, the microscopic theory of Heisenberg magnets faces a fundamental difﬁculty because the state with the strict antiparallel spin alignment is not a true ground state of the system in the presence of an antiferromagnetic exchange interaction. At a ﬁnite temperature T , the quasi-particles that destroy antiferromagnetic order are magnons (spin waves). The existence of several sublattices leads to the existence of several branches, one for each sublattice, of spin waves. Two of them are quasi-acoustic, and the rest are of the exchange

type. The quasi-acoustic spin waves satisfy a linear dispersion law. In most antiferromagnetic materials, however, their spectrum has an energy gap, with the width determined by the expression ω = μB (2B A B E )1/2 , where μB is the Bohr magneton. The existence of the linear dispersion law is conﬁrmed by the linear temperature dependence of the speciﬁc heat, and more reliably by inelastic neutron scattering. Fig. 3 shows the spin wave dispersion relationships of MnF2 . In the scale used, the gap is barely observable. The gap in the spin wave spectrum is studied by means of antiferromagnetic resonance without any particular difﬁculties in easy-plane antiferromagnets where an almost gapless branch is observed, in addition to the magnon branch with a large gap (≈μB (2B A B E )1/2 ). The study of this nearly gapless branch allows the subtle effects of the dynamic interaction of the spin system with other degrees of freedom of the crystal (phonons, oscillations of nuclear spins, etc.) to be revealed. This becomes possible because of the “exchange ampliﬁcation” of the frequency of coupled vibrations in antiferromagnets. Branches of the exchange spin waves are relatively less studied; spin-wave analogues of optical phonons have a wide gap ≈μB B E , and rather weak dispersion. Many antiferromagnetic materials are transparent in the optical and infrared regions. The distinctive features of the optical properties of antiferromagnetic materials are the abnormally high spontaneous magnetic birefringence arising in the easy-plane, and the change of birefringence in the easy-axis antiferromagnetic materials. Singlemagnon scattering also turns out to be stronger

80

ANTIFERROMAGNETISM VECTOR

than what could be expected from the magnetic dipole–dipole transitions alone. Exciton–magnon excitations are observed in the absorption spectra. ANTIFERROMAGNETISM VECTOR A macroscopic parameter of antiferromagnets and ferrimagnets; the order parameter at the magnetic phase transition to the antiferromagnetic state (see Antiferromagnetism). The vector of an-

tiferromagnetism is deﬁned as such a linear combination of the magnetization vectors M α of individual magnetic

sublattices, that it differs from a sum M = kα=1 M α which deﬁnes the total magnetization, where α = 1, 2, 3, . . . , n, and n is the number of sublattices. To describe the atomic magnetic structure, n − 1 antiferromagnetism vectors Li are introduced. The expression for Li depends on the magnetic structure, e.g., in the simplest two-sublattice antiferromagnet (or ferrimagnet), only one such antiferromagnetism vector exists, L = M 1 − M 2 . Sometimes, normalized antiferromagnetism vectors are used, l = L/|L|, l 2 = 1. It is possible to write dynamic equations for the antiferromagnetism vector to deﬁne linear and nonlinear spin waves in antiferromagnets and ferrimagnets (see Landau–Lifshits equation). ANTIFRICTION MATERIALS

Materials having low values of the friction coefﬁcient. Besides low values of the friction coefﬁcient (0.004–0.10 with lubricant, and 0.12–0.20 without lubricant), antifriction materials are characterized by considerable wear resistance, adequate mechanical strength and plasticity, corrosion resistance, and absence of sticking. These materials slightly wear the adjoining surfaces. Depending on the operating conditions antifriction materials with special properties are created to be used with lubrication by oil or water, without a lubricant, in the atmosphere or in vacuo, at a high temperature, in chemical environments, etc. Classiﬁed among antifriction materials are the following: cast materials (babbitts, bronzes, and brasses); baked ones manufactured by powder metallurgy, including composite materials on the base of iron or bronzes; combined (mostly metal-ﬂuoroplastic) materials; antifriction cast irons and antifriction steels (copper steel, graphitized steel). The cast

antifriction materials are manufactured by melting source components with subsequent casting. As to the structure type, they are subdivided into those with harder inclusions of intermetallic compounds placed in a relatively light matrix (e.g., aluminum bronze, tin bronze, tin babbitt), and those with soft inclusions with metallic structural components in a stronger solid solution matrix (e.g., lead bronze, aluminum alloys containing tin, lead and cadmium). A typical feature of baked (metalloceramic) antifriction materials is the presence of pores (8–27% of the volume) which are impregnated with a ﬂuid lubricant. The metallic base of such materials is iron, steel, copper, bronze, and nickel. In addition to these, baked materials contain components (graphite, sulﬁdes, selenides and others) to serve as a dry lubricant. Baked antifriction materials in most cases have higher tribotechnical properties than the ones obtained by casting, and can provide unique properties unattainable in cast alloys. ANTIMONY (Lat. stibium), Sb

A chemical element of Group V of the periodic system with atomic number 51 and atomic mass 121.75. It is related to As and Bi in its properties. Natural antimony has 2 stable isotopes Sb121 (57.25%) and Sb123 (42.74%). Important radioactive isotopes are Sb122 (T1/2 = 2.8 days), Sb124 (T1/2 = 60.2 days), Sb125 (T1/2 = 2.0 years). Electronic conﬁguration of the outer shell is 5s 2 5p3 . Successive ionization energies are 8.64, 16.5, 25.3, 44.0, 55.4 eV. Atomic radius is 0.161 nm; radius of Sb3+ ion is 0.090 nm, of Sb5+ 0.062 nm, of Sb3− 0.208 nm. Work function is 4.08 eV. Oxidation states are −3, +3, +5. Electronegativity is ≈2.0. Antimony is a silvery-white metal with strong brilliance. In a free form antimony exists in several crystalline and amorphous modiﬁcations. Under normal conditions, the rhombohedral crystalline modiﬁcation is stable with parameters a = 0.45064 nm and α = 57.1◦ . Under increased pressure the cubic and hexagonal modiﬁcations appear. Besides, three amorphous modiﬁcations are known: yellow, black and explosive ones. The rhombohedral modiﬁcation is characterized by gray star-like crystals. For this modiﬁcation the density is 6.690 g/cm3 ; Tmelting = 903.5 K,

ANTISCREENING FACTOR

Tboiling = 1907 K. Heat of melting is 20 kJ/mole, heat of evaporation is 124 kJ/mole; speciﬁc heat cp = 25.2 kJ·mole−1 ·K−1 . Thermal conductivity is 18.84 W·m−1 ·K−1 , temperature coefﬁcient of linear expansion of polycrystalline antimony is 9.2·10−6 K−1 (at 273 K), 10.3·10−6 K−1 (at 873 K). Debye temperature is 204 K. Brinell hardness of technical grade antimony is 320 to 580 MPa; of zone reﬁned antimony it is 260 MPa. Shear modulus is 20 GPa, normal elasticity modulus is 56 GPa. Antimony is a diamagnet; magnetic susceptibility of polycrystalline antimony is 0.81·10−9 (at 293 K); electrical resistivity 0.39 μ·m (273 K), temperature coefﬁcient of electrical resistivity is 5.1·10−3 K−1 . Compounds of antimony with indium, gallium, aluminum, cadmium and other metals (so-called antimonides) possess semiconductor properties, with indium antimonide InSb possessing the highest carrier mobility among all known semiconductor materials. Antimony is also used as a component of various alloys, it is contained in lead storage battery plates (4 to 12% by mass). Antimony oxide Sb2 O3 is introduced into the composition of glasses characterized by a low refractive index. ANTIREFLECTION COATING OF OPTICAL ELEMENTS

A means of increasing light transmission of optical elements by coating their surfaces with nonabsorbtive lm s. The optical paths through such ﬁlms should be comparable to the radiation wavelength. Without an antireﬂection coating the loss of light during reﬂection from their optical surfaces may reach 10% or more. The antireﬂection effect involves interference of light beams reﬂected from the front and back sides of the dielectric layers that form the coating. Provided the angles of incidence remain close to normal the antireﬂection coating has a maximum effect. The thickness of the thin coating ﬁlm should be an odd number of quarter wavelengths, and the refractive index of the ﬁlm, n2 should satisfy the relation n22 = n1 n3 , where n1 and n3 are the indices of refraction of the two media adjacent to the ﬁlm (the ﬁrst is often air, n1 = 1). For optical elements made of glass with a low value of n2 a single layer antireﬂection coating is often insufﬁcient, whereas

81

two-layer coating ﬁlms almost totally eliminate ree ction of light from the surfaces of the optical elements. Note that this is true in a rather narrow spectral range only. To attain antireﬂection protection over a broad spectral range triple and multiple layer coating systems are commonly used. Antireﬂection coating plays a very important role in lowering optical losses in multilens optical systems, in laser technology where coating makes it possible to lower feedback losses from the optical cavities, in opto-acoustic instruments, etc. ANTIRESONANCE, MAGNETIC See Magnetic antiresonance. ANTIRESONANCE, OPTICAL See Optical antiresonance. ANTI-SCHOTTKY DEFECT A two-component defect in crystals of binary

(MX) or more complex composition. Its components are IM and IX , the amounts of interstitial atoms of chemical elements M and X which themselves constitute the regular lattice of the crystal. Anti-Schottky defects can be equilibrium stoichiometric defects arising at elevated temperatures, e.g., because of “vaporization” of M and X atoms from the surface to the inside of the MX crystal. The creation of anti-Schottky defects is hampered by the necessity of inserting the larger M and X atoms into the smaller-sized interatomic “cavities” (i.e. interstitial sites). These defects have the name anti-Schottky because a Schottky defect is a vacancy formed by transferring an atom from the bulk of the crystal to its surface. ANTISCREENING FACTOR

A parameter characterizing antiscreening (the phenomenon which is inverse to electric charge screening). If P0 is a response arising as a result of some inﬂuence in the absence of a medium, and P is the same response in the presence of the medium, then one can write P = P0 (1 − γ ). If the dimensionless parameter γ is less than zero it is commonly referred to as an antiscreening factor. The Sternheimer antiscreening factor (R.M. Sternheimer, 1951) γ S describes the enhancement of an intracrystalline electric ﬁeld gradient at a nucleus

82

ANTISITE DEFECT

due to the polarization of closed atomic shells by external electric charges. The value of |γ S | can be rather large (50–100). ANTISITE DEFECT

An atom of one sublattice of a two- or multicomponent crystal, occupying a site of another sublattice; actually, a substitutional atom, denoted as XM (atom X at a site of sublattice M). Adjacent defects XM and MX represent an antistructural defect pair. For unequal concentrations of MX and XM the antisite defects determine an excess of component M or X, i.e. a deviation from stoichiometric composition. ANTI-STOKES LUMINESCENCE Photoluminescence, or luminescence at wave-

lengths less than that of the exciting light, which is in contradiction with Stokes’ rule. Anti-Stokes luminescence is common in the region of overlap between the excitation and the luminescence wavelengths. The emission of a quantum with an energy exceeding that acquired in the absorption occurs due to the additional involvement of the thermal motion of the luminescent system. This results in the Vavilov law, which reﬂects the fact that the probability of such a process decreases rapidly as the involved energy rises, and it depends on the thermal motion intensity (temperature). Of greater importance are the fundamental violations of Stokes’ law when the emitted luminescence lies in the region of wavelengths less than that of the exciting light. Such effects are possible by making use of several exciting light quanta (most often, of two) in the emission process, by the simultaneous absorption of two photons by one electron at a high excitation intensity, by sequential absorption of two quanta by the electron, and by pooling the energy of two excited electrons to produce the emission (cooperative luminescence), etc. ANTI-STOKES RAMAN LINES Lines in the spectrum of Raman scattering of light that are located on the high-frequency side of

the exciting line. Anti-Stokes light scattering lines are caused by annihilation of the excitation quantum in the system by the inelastic scattering of an incident photon on it (a phonon, magnon, plasmon, etc., is typically annihilated in a crystal). The intensity of

anti-Stokes lines depends on the initial level population (excited) and decreases with a lowering of the temperature. The presence in a spectrum of Stokes and anti-Stokes pairs of lines, symmetric relative to exciting one, is often used to discriminate between the processes of Raman scattering and luminescence, while their intensity ratio characterizes the scattering medium temperature. ANTISTRUCTURAL DEFECT A defect in a binary or more complex crystal

containing two chemical elements M and X. The defect consists of two components – substitutional atoms MX (atom M at site X) and XM (atom X at site M). The formation of antistructural defects in a nonmetallic crystal can be accompanied by changing the charge state of its components. For example, atoms M and X in the normal positions at their “own” sites MM and XX can be neutral, while as components of an antistructural defect, if M is a metal, MX tends to become an acceptor and X (metalloid) a donor XM . Antistructural defects either exist in the equilibrium state at elevated temperatures (e.g., in crystals Bi2 Te3 , Mg2 Sn, and others) or are created as nonequilibrium metastable defects, e.g., as a result of nuclear radiation (see Antisite defect). ANTISYMMETRIC VIBRATIONS of crystal lattice Normal vibrations which reverse their sign un-

der the application of an appropriate symmetry operation (see Crystal symmetry). In ionic crystals antisymmetric vibrations involve a change of the electric dipole moment. ANTISYMMETRY of crystals, Shubnikov symmetry One of the particular cases of colored symmetry (hypersymmetry). In ordinary crystal symmetry, only spatial (position or orientation) symmetry

is considered, while in hypersymmetry, another attribute (conventionally, color or spin direction) is assigned a value at every point of the crystal. If the additional attribute can take on only two alternative values (black and white), such a particular case of hypersymmetry is referred to as antisymmetry, in other words as black and white symmetry. If there are many values then one speaks

ARMCO IRON

about color symmetry. Another term for antisymmetry is Shubnikov symmetry after A.V. Shubnikov who introduced the concept. In analogy to the ordinary crystal symmetry groups, there exist 122 point, 36 translational and 1651 space Shubnikov groups. All of them have been derived and classiﬁed, a system of notation has been developed, and they are used in concrete physical studies. Examples of the physical realization of crystal antisymmetry can vary. Treated as the color change operation may be, for example, a change in the chemical type of atoms in an ordered binary alloy, or in the sign of the displacement of atoms and of the electric charge, and others. Solid state physics makes the widest use of this approach for the Shubnikov classiﬁcation of the magnetic symmetry of crystals, where the color change operation has the sense of the time inversion operation R, and, as a consequence, the inversion of the magnetic moments and magnetic elds (see Magnetic symmetry group). Operations of antisymmetry, which occur in magnetic crystal symmetry and are combinations of rotation or translation with R, are referred to as antirotations and antitranslations. ANYONS (fr. any)

Particles that obey a statistics which is intermediate between the Bose (see Bose–Einstein statistics) and Fermi (see Fermi–Dirac statistics) types. Such particles can exist in two-dimensional space since the topology of this space admits the presence of indeterminate wave functions for (identical) particles a with strong short range repulsion (hard core). These functions obey the permutation rules Pj k ψ = exp(iπα)ψ , where Pj k means the permutation of j th and kth particles, and α is any real number which is sometimes called a statistical parameter. The value α = 0 corresponds to bosons and α = 1 denotes fermions (see Second quantization), while intermediate values are indicative of an intermediate statistics. The possibility of the existence of an intermediate type statistics was ﬁrst pointed out by J.M. Leinaas and J. Myrheim (1977), and the term “anyon” was introduced by F. Wilczek (1982). Intermediate statistics can also be obeyed by particles in one-dimensional space (to which a term “anyon” is inapplicable, as a rule), and by distinguishable particles (anyons of

83

many types). The permutation conditions for the latter have the form Pj2k ψ = exp(iπα)ψ , and at α = 0, 1 one can speak about an in-between statistics. The ambiguous nature of anyon wave functions results in the fact that the quantum-mechanical problem of many anyons cannot be solved even for the simplest case when there is no interaction. The usual procedure of seeking solutions in terms of single-particle wave functions is not applicable here. The statistics of all elementary particles is determined by their spin in accordance with the Pauli principle. Therefore (since real space is threedimensional), elementary particles with an intermediate statistics cannot exist in free space; this statistics can be valid only for quasi-particles in quasi-two-dimensional and quasi-one-dimensional systems. In particular, the elementary excitations in the fractional quantum Hall effect (see Quantum Hall effect) obey intermediate statistics, i.e. they are anyons. At a ﬁlling factor ν = 1/q where q is an odd integer, the statistical parameter of these excitations is α = ν. The appearance of the effect at ﬁlling factors ν = p/q kept constant is explained quite well in the framework of so-called hierarchic theory. This implies that there appear excitations over a “primary” electron gas that represent the anyon gas. Other excitations can arise which also represent the anyon gas but with another statistical parameter, and so on inﬁnitely. One can demonstrate that under particular conditions an anyon gas is a superconductor. As far as it is known high-temperature superconductivity is of a quasi-two-dimensional nature, and an hypothesis about an anyon mechanism of superconductivity has been suggested, but there is no experimental conﬁrmation of it. See also Anderson mechanism of high-temperature superconductivity. APW METHOD See Augmented plane waves method. ARMCO IRON (ARMCO is an acronym of American Rolling Mill Corporation) Highly puriﬁed iron with high plasticity, enhanced electrical conductivity, high magnetic saturation and resistance against corrosion. ARMCO iron falls into soft magnetic materials, its magnetic

84

AROMATIC COMPOUNDS

properties depending upon the quantity of impurities, sizes of crystal grains, elastic and plastic stresses. ARMCO iron is used for the manufacture of electrical engineering products to be operated in constant and slowly varying magnetic ﬁelds. In metallurgy, it is employed as the basic element in the manufacture of many magnetic alloys and as the charge in the production of alloyed steel. AROMATIC COMPOUNDS

A group of organic compounds possessing a system of conjugated π -bonds. The term originated from the speciﬁc odor of natural substances containing aromatic compounds. These compounds are exempliﬁed by the polycyclics – benzene (C6 H6 ), naphthalene (C10 H8 ), anthracene (C14 H10 ), tetracene (C18 H12 ), pentacene (C22 H14 ), and others, with a common formula C4n+2 H2n+4 , where n is the number of benzene-type rings. The molecules of polycyclics are planar and form molecular crystals in the solid phase. Most of them belong to the monoclinic system with two molecules in a unit cell. Electronic properties of aromatic compounds are determined mainly by pz electrons of C atoms forming a delocalized π -orbital. The π -electrons excited by light undergo a π –π ∗ transition and account for the absorption spectral shift from the ultraviolet to the visible part of the spectrum in the above-indicated sequence of polyacenes. The mobility of π -electrons determines important physical and chemical properties of aromatic compounds: photoconductivity of their crystals, migration of electron excitation energy, catalytic activity. Aromatic compounds are model systems for organic semiconductors. The dark electrical conductivity of pure crystals is low, σ ∼ 10−2 –10−12 −1 cm−1 . The typical mobility of excess electrons and holes moving in narrow bands takes on values of the order of 1 cm2 ·V−1 ·s−1 . ARRHENIUS LAW (S. Arrhenius, 1889)

Relation stating the temperature dependence of the reaction rate constant K U , K ∼ K0 exp − RT where U is the activation energy of the reaction, and R is the universal gas constant. The parameter

Activation energies U1 and U2 for a double minimum potential.

K0 has a temperature dependence weaker than exponential. The value of K is determined from the expression for the reaction rate nA+mB+lC+· · · which is proportional to the product of the appropriate powers of concentrations (denoted by brackets): v = K[A]n [B]m [C]l · · · . The Arrhenius law was deduced empirically and can be justiﬁed from the Boltzmann distribution. The ﬁgure schematically presents the dependence of the energy of the reacting particles on their generalized coordinate. The activation energies U1 of the reaction 1 → 2 and U2 of reaction 2 → 1 are determined by the energies of the initial states 1, 2 and the height of the potential barrier separating them. The barrier energy U varies from several electron-volts to almost zero; it can equal zero, e.g., in ionicmolecular reactions or in the reactions with mechanisms based on the tunnel effect. Such reactions can occur at temperatures close to absolute zero. Reactions in solids with participation of the inherent and impurity atoms, conduction electrons, and various quasi-particles also follow the Arrhenius law. In them, a part of the activation energy U D can arise from the diffusion of reagents, determined by the temperature dependence of the diffusion coef cient D = D0 exp(−U D /RT ). See also Interdiffusion, Activation energy, Thermal activation. ARTIFICIAL EPITAXY See Amorphous epitaxy.

ASTERISM

ASBESTOS (fr. Gr. ασβεσ τ oς , unquenchable) Fine-ﬁber minerals capable of splitting into

ﬂexible and thin ﬁbers (up to 0.5 μm thick). The most signiﬁcant is serpentine asbestos. There are such varieties as chrysotile-asbestos and picrolite. Chrysotile-asbestos Mg6 Si4 O10 (OH)8 has a lamellar-tubular structure with a monoclinic lattice. Felted and parallel-ﬁber aggregates are typical of it. The cleavage is imperfect along (110) at the angle 130◦ . Density is 2.5 to 2.65 g/cm3 . Mohs hardness is 2.0 to 3.0. Impurities: Fe (up to 3%), Ca, Mn, Ni, Al, Na. Water content is 13.0 to 14.8%. Refractive indices: ng = 1.522 to 1.555; np = 1.508 to 1.543. The ﬁbers of asbestos are rupture-strong (285 to 365 kg/mm2 ). Asbestos is ﬁreproof (T melting is 1500 ◦ C); it has high sorption ability (see Sorption), swelling ability; it conducts heat poorly; it is stable against alkalis; upon heating, it loses water and transforms to forsterite. Asbestos is used in textile, cement, paper, radio industry, road surfacings, etc. ASCENDING DIFFUSION

A process of transport, whereby the ﬂow of particles is directed along the concentration gradient. In contrast to conventional diffusion, in this case the difference in concentration of the diffusing component does not diminish but rather grows. The possibility of ascending diffusion arises from the fact that the driving force of the diffusion is the gradient of the chemical potential which, in general, can differ from the concentration gradient. Different ﬁelds which contribute to the chemical potential in addition to the entropy of mixing, can cause the ascending diffusion; examples are thermal ﬁelds (thermodiffusion), electrical ﬁelds, vacancy ﬁelds, phase non-uniformity of the material, and the ﬁeld of elastic stresses. These ﬁelds make the potential barrier that the diffusing particle encounters an unsymmetrical one, and the result is a preferred drift in the direction of the ﬁeld. In a general phenomenological theory ascending diffusion can be described in a systematic uniform manner, but the detailed mechanisms operating in the above mentioned cases are different. The Gorsky effect (V.S. Gorsky, 1935), which involves ascending diffusion caused by local gradients of elastic stresses in crystals, is speciﬁc for solids. For example, during the bending of a plate

85

made of metal alloys the concentration of atoms with the greater atomic radius grows at the exterior side of the ﬂexure (a partial stress relaxation accompanies this process). By providing for the segregation of atoms of different types, ascending diffusion, evidently, plays an important role in the phase separation in alloys, and at the formation of atmospheres of the impurity atoms in the strained regions of a crystal, e.g., interstitial atoms preferentially concentrate in the stretched region of the ﬁeld of stresses at dislocations (see Cottrell atmosphere). ASPEROMAGNET An amorphous magnetic substance in which the random frozen magnetization mi has a ﬁrst

moment M = mi c and two second moments, 2 q = (mi )2 c and q⊥ = (m⊥ i ) c . The averaging is performed over conﬁgurations, the indices and ⊥ denoting projections of mi onto the vector M or onto the plane perpendicular to M, respectively. The asperomagnetic state is observed in two types of amorphous magnetic materials: in alloys and metallic glasses containing rare-earth elements and noble metals, such as DyCu, TbAg; in systems of the spin glass type. In the ﬁrst case, the origin is the large value of the magnetic anisotropy constant (typical of rareearth elements) and the random orientations of the anisotropy axis (typical of alloys and glasses). In the second case, the cause is the presence of concurrent random ferro- and antiferromagnetic interactions. Asperomagnets often exhibit nonergodic behavior (see Nonergodicity). ASTERISM

The characteristic oblong shape of X-ray diffraction spots from deformed monocrystals exposed to X-radiation of a continuous type. In the case of transmission images (Laue patterns), the diffraction spots are elongated toward the center of the picture. Asterism arises due to the reﬂection of the X-ray beam from the bent part of a crystal. The horizontal diameter of the spot in angular units is ϕ1 = 2α and the vertical one is ϕ2 = −2α sin θ , where θ is the Bragg angle (see Bragg law) and α is the ﬂexure angle of the reﬂecting plane. At small θ , ϕ2 ϕ1 which explains elongation of spots at asterism, and proves that the

86

ATHERMIC CREEP

length of asterism bands can serve as a measure of e xure. In reﬂection imaging (epigrams), the directional stretching of diffraction spots is observed according to the ﬂexure axis orientation relative to the initial beam. ATHERMIC CREEP

A type of low-temperature logarithmic creep, independent of temperature. Its rate after the instant jump of the initial strain ε0 at the moment of load application quickly decreases in time, ε = α/t . Typical for this creep is the time dependence of strain caused by the motion of dislocations, ε = ε0 + α ln(νt + 1), α and ν being constants. A feature of athermic creep is the smallness (0.1 to 1%), in comparison with ε0 , of the strain under creep. The deceleration of athermic creep is associated either with the increasing density of support of intersecting dislocations or with the “depletion” of mobile dislocations. At temperatures close to absolute zero (∼1 K), the barriers of the support type are overcome with the help of a quantum-mechanical tunnel effect (see Lowtemperature yield limit anomalies). According to Mott, in this case α is independent of temperature, α ∝ 2πh/(2Mu)1/2 , where h is the Planck constant, M is the effective mass of dislocations, u is a quantity on the order of the energy of the step transformation at the dislocation (3·10−19 J). Within the range of temperatures between 1 K and T ∼ 0.1Θ, where Θ is the Debye temperature, the crossing of the support may be activated by zeropoint vibrations of dislocation segments. The factor 2 T 1 kBΘ 1+ α= 2 hν Θ insigniﬁcantly changes with temperature at T < Θ. The value of ε at the athermic creep is not large, but it needs to be accounted for in the operation of precision parts and products. ATHERMIC PLASTICITY

Lack of sensitivity of the characteristics of a plastic deformation process of a solid to changes

in temperature. Athermic plasticity characterizes the regularities of plastic deformation of crystals at low and

very low temperatures. It emphasizes that the thermoactivating character of elementary dislocation processes in determining the deformation kinetics, such as overcoming Peierls barriers by dislocations (see Peierls–Nabarro model) or local barriers determined by the defects of crystalline structure, is of limited applicability for the description of low-temperature plasticity. Athermic plasticity is not fully understood; it has been proposed as (i) playing a crucial role in quantum ﬂuctuations that arise during the motion of dislocations through barriers, and (ii) playing a role in the replacement of a thermoactivated barrier penetration by an activation-free process of the overbarrier motion, which occurs owing to the high level of effective forces acting upon dislocations, and the low level of dynamic friction restraining the dislocations (see Internal friction), typical for low-temperature deformation. ATMOSPHERE See Cottrell atmosphere, Snoek atmosphere, Suzuki atmosphere. ATOM

An atom consists of a positively charged nucleus with a size on the order of 10−15 m and a surrounding electronic cloud with a size of about 10−10 m (see Atomic radius). An atom as a whole is electrically neutral; the positive charge of the nucleus Ze (Z is the atomic number and e is the elementary electron charge) is compensated by the negative charge of its Z electrons. An atom can accept or donate one or more electrons to become, respectively, a negatively or positively charged ion. The complicated structure of the electron cloud is determined mainly by Coulomb interactions, the attraction of electrons to the nucleus and their mutual repulsion, as well as by the Pauli exclusion principle. Relatively small but fundamentally important contributions to the energy arise from the spin–orbit interaction and the spin–spin interaction. A single-electron approximation is widely used to describe an atom: the wave function of the electrons is a product of one-electron wave functions (Hartree method) or a linear combination of such products which satisﬁes the requirement of interchange invariance (Hartree–Fock method).

ATOMICALLY CLEAN SURFACE

In this approximation one can speak about oneelectron energy levels and corresponding electron shells of an atom. To describe them approximately, the model of a hydrogen-like atom is employed, with the shells characterized by the principal quantum number n = 1, 2, 3, . . . , and their substructure by the orbital quantum numbers l = 0, 1, 2, . . . , n − 1 and m = 0, ±1, . . . , ±l. The electrons of the K-shell with n = 1 are closest to the nucleus with the deepest (most negative) energy levels. Then follow the L, M, N, . . . shells with n = 2, 3, 4, . . . . In the ground states of the atoms H and He only the K-shell is occupied. As Z grows, the orbits with higher quantum numbers become ﬁlled. The electron conﬁguration of an atom is speciﬁed by symbols that indicate the values of quantum numbers n and l of ﬁlled shells in ascending order, and the number of electrons in them; the values l = 0, 1, 2, 3, 4, . . . being denoted with corresponding letters s, p, d, f, g, . . . . For example, the conﬁguration 1s 2 2s 2 2p6 of the neon atom has two electrons with n = 1 and l = 0, plus two electrons with l = 0, and six electrons with l = 1 at n = 2. Each l shell contains 2(2l + 1) electrons when it is full. Another approximate method for describing an atom (Thomas–Fermi method) is based upon a structureless cloud of atomic electrons with their density distribution determined by the Poisson equation. The outer valence electrons determine the chemical properties of atoms, their ability to form this or that compound, the structure, binding energy, and other characteristics of compounds. Although atoms are the structural elements of solids, the distribution of the atomic electrons in a solid differs from that of a free atom. The conﬁgurations of valence electrons undergo considerable changes, depending on the type of bonding force between atoms, the number and positions of nearest neighbors, etc. In a crystalline solid, the states of valence electrons depend on whether the atoms occupy sites of the regular lattice, or they are doping atoms or substitutional atoms. The presence of the two latter types introduces additional levels in the energy spectrum of electrons in crystals and inﬂuences the optical, electrical and other properties of a crystal. The inner atomic shells also undergo some change, but to a much lesser extent. This

87

is substantiated by data of X-ray emission spectroscopy, by the observed differences of characteristic X-ray frequencies for the inner shells of atoms of a given chemical element incorporated into different chemical compounds. It is not feasible to solve exactly the problem of the states of atoms forming (comprising) a solid. The approximation often used in condensed matter theory is based on reducing the number of independent variables per atom down to 3. Here, the atom is represented as a structureless entity, while interactions involving atoms are described by various, mostly empirically chosen, potentials with limited applicability (see Interatomic interaction potentials). In a more precise approach the valence electrons are singled out, and the nucleus with the deep electron shells is treated as a point particle with an effective charge. The potential of an atom is determined by the distribution of its electron density. An approaching test particle perturbs this distribution in a manner that depends on its nature and its speed relative to the atom. Atom–atom potentials differ for different pairs of atoms. In the quantum description one cannot speak about each particular electron being afﬁliated with one particular atom of a solid. The delocalization of electrons among many atoms causes the splitting of atomic energy levels and the creation of bands of allowed energies in crystals. Such broadening is rather small for electrons in deep levels. For those in outer atomic shells, broad (several electron-volts) allowed energy bands arise, and are particularly prominent in metals, with their structure determining the electric, optical, and other properties of the crystal. ATOM DISPLACEMENTS See Static displacements of atoms, Thermal displacements of atoms. ATOMICALLY CLEAN SURFACE

A surface free of impurities and having a pristine crystal structure. To obtain and preserve an atomically clean surface, various methods of cleaning in a super-high vacuum (10−8 Pa) are used. The main methods are high temperature heating, bombardment with ions of noble gases with annealing and chemical pretreatment to obtain products that are removable at

88

ATOMIC CHARGE

moderate temperatures. An absolutely clean surface is impossible to obtain: the sources of contamination are the impurities in a crystal bulk and the adsorption of particles from residual gases. Therefore, the surface is considered to be clean, if the concentration of impurities is so small that it fails to affect phenomena under study. Auger electron spectroscopy is the most suitable method of monitoring surface cleanliness (the sensitivity is 10−2 –10−3 monolayers). The investigation of an atomically clean surface structure is performed by low-energy electron diffraction and high-energy electron diffraction methods (see Electron diffraction). From an analysis of the data from structural investigations, the atomically clean surfaces of crystals, especially semiconductor ones, can be reconstructed. Surface structures can form with periods other than those in atomic planes in a crystal bulk parallel to the surface. A special notation is adopted for these surface structures. They include the chemical symbol of the crystal, the orientation of a face, and the ratio of the unit cell vectors of surface structure to the corresponding vectors in the bulk, e.g., Si (111) – 7 × 7, Au (100) – 5 × 1 and so on. According to modern concepts, the cause of the reconstruction of the upper atomic planes of a crystal is the tendency to reduce the excessive free energy of a surface lattice relative to that in the bulk. The supposition that the reconstruction is determined by the uncontrollable contamination of a surface failed to be conﬁrmed experimentally. The difﬁculties connected with clariﬁcation of the nature of surface reconstruction are complicated by the fact that the problem of the determination of the coordinates of the unit cell atoms for the surface structures with large unit cells is yet to be solved because of the complexity of the calculations in the structural analysis. Therefore, various hypothetical models are used in discussions of this reconstruction, their ability to approximate reality being tested using data obtained by various methods. All the varieties of models can be divided into two classes: those based on small static displacements of atoms from their normal positions in the surface lattice, and those involving the concept of orderly-spaced defects at the surface (vacancies, adatoms, etc.). There has been considerable progress in understanding surface structures

because of data obtained from scanning tunneling microscopy. According to estimates based on different data, the reconstruction encompasses several atomic planes of a crystal. There are only a limited number of orientations of planes which coincide with atomic planes having the same crystallographic indices and characteristic surface structures. Such surfaces are referred to as atomically smooth. In other cases, energy can be gained by the decay of a ﬂat surface to micro facets, or by the formation of a stepped surface including terraces of low-index facets connected by equispaced atomic steps as high as one or more interplane distances. Besides the structure, there are also other important properties of a surface such as the electronic energy band structure and dynamical characteristics (frequencies of atomic vibrations, their vibration amplitudes) that are different from the analogous properties in the bulk. Therefore, the near-surface region is considered as a special surface phase with its own conditions of equilibrium. The atomically clean surfaces of some crystals of semiconductors and metals with particular orientations are the place where order–disorder phase transitions as well as order–order ones occur, while there are no phase transitions in the bulk. The order–order reconstruction can occur as transitions between surface structures, both with unit cells lying in one plane, and with changes of facet structure – morphological transitions. ATOMIC CHARGE See Effective atomic charge. ATOMIC FORM FACTOR

A parameter of the elastic scattering of a plane wave (X-ray, electron, neutron) by an isolated atom, which determines the amplitude of the scattered wave as a function of the scattering angle. In the scattering of waves in crystals, the amplitudes of scattering by individual atoms are ampliﬁed in some directions, while they are decreased in others; the total result being determined by the values of the atomic form factors of the atoms forming the crystal. A general expression for an atomic form factor is f (s) = K ρ(r) exp(is · r) dr ,

ATOMIC MAGNETIC STRUCTURE

89

types that correspond to ferromagnetism, antiferromagnetism, and ferrimagnetism.

Atomic form factor.

where s = k − k 0 , and k 0 , k are the wave vectors of the incident and scattered waves, respectively (see Fig.), and K is a factor dependent on the type of radiation. The X-ray scattering is determined by the electron density ρ X = |ψ(r)|2 , and values of f X (s) are on the order of 10−11 cm. The electron scattering is determined by the electrostatic potential of the atom ϕ(r); ρ el (r) = ϕ(r), with values of f el (s) of the order of 10−8 cm. Neutron scattering may be thought of as taking place at the point potential of the atomic nucleus, with values of f n (s) of the order of 10−12 cm, and no angular dependence. ATOMIC MAGNETIC STRUCTURE

Position and spatial orientation of atomic magnetic moments, or of the magnetic moment density of delocalized electrons (the latter pertains to band magnetism). The presence of a magnetic structure in a material implies that the time averages of the above quantities differ from zero. These averages are zero in materials having no magnetic structure (an external magnetic ﬁeld is presumed absent). The emergence of a magnetic structure in a material is always accompanied by symmetry lowering, if for no other reason than that the time reversal operation is not a symmetry transformation. In this connection, the state of a material exhibiting a magnetic structure is called a magnetically ordered state, and the process of transforming to a magnetically ordered structure is a magnetic phase transition of the disorder-to-order type. A magnetic structure is commonly found in those crystalline substances where the magnetic atoms tend to occupy symmetrical crystallographic sites, while the mean magnitudes of atomic magnetic moments are oriented in a deﬁnite manner with respect to one another and to the crystallographic axes. The magnetic structure of most magnetic crystals can be classiﬁed as one of three basic

A ferromagnetic structure refers to one with all the magnetic moments aligned in the same direction. This structure is characterized by the magnitude and direction of the magnetization M. The simplest antiferromagnetic structure is a set of two interpenetrating magnetic sublattices, with their respective magnetization vectors, M 1 and M 2 , equal in magnitude and opposite in direction, viz., the net vector M = M 1 + M 2 is zero. The two-sublattice antiferromagnetic structure is described by the magnitude and direction of the antiferromagnetism vector, L = M 1 − M 2 . The condition M 1 = −M 2 necessarily assumes that atoms belonging to different magnetic sublattices are the same, and their crystallographic positions are equivalent, since a difference in the magnetic moments inevitably results from the dissimilarity of the atoms, or their positions. More complicated antiferromagnetic structures have been discovered in many crystals. For example, in Mn3 NiN, the magnetic moments are directed along the sides of an equilateral triangle (a non-collinear antiferromagnetic structure with three sublattices), while in YMnO3 , they follow the directions of the sides of two equilateral triangles rotated by 60◦ relative to one another (a six-sublattice structure). Noncoplanar antiferromagnetic structures are also encountered, e.g., the magnetic moments in the foursublattice antiferromagnet UO2 lie along the body diagonals of a cube. Any particular magnetic structure of the ferroor antiferromagnetic type forms in a substance as a result of electrostatic exchange or direct interactions, with the exchange interactions far exceeding, as a rule, those of the direct type (i.e. magnetic dipole interactions and spin–orbit interactions). In quite a number of materials exchange interactions establish an antiferromagnetic structure (a bi- or polysublattice one), whereas the other interactions (see Dzialoshinskii interaction) bring about a small distortion of this structure, which causes a nonzero ferromagnetism vector, M L, to appear. Such materials are called weak ferromagnets, and the corresponding magnetic structures are called weak ferromagnetic structures. The competition of the strong electrostatic and weak direct forces may also have other conse-

90

ATOMIC ORBITALS

quences i.e. it may produce a long-period modulated magnetic structure in a crystal. Here, the exchange forces order the magnetic moments according to either a ferro- or antiferromagnetic pattern, while the relativistic forces lead to the vectors M = M(ξ ) or L = L(ξ ) gradually changing along a certain direction ξ that is called the axis of the modulated structure. In the simplest modulated structures, M (or L) just rotates around the axis (long period helices); there are also more complicated modulated magnetic structures. The formation of a magnetic helix in some crystals is due to the exchange interaction. The helix period is of the same order of magnitude in this case as the distance between neighboring magnetic atoms. A magnetic helix differs fundamentally from a noncollinear antiferromagnetic structure (e.g., of YMnO3 type) in that the angles between the magnetic moments may not correspond to 360◦ /n values (n = 1, 2, 3, . . .). The helix period is not commensurate with the interatomic distances ξlm in this case. Another common type of magnetic ordering (ferrimagnetic structure) occurs in ferrimagnets, where the exchange forces position the atomic magnetic moments in a manner resulting in nonzero values of both M and L. In particular, a ferrimagnetic structure appears when the magnetic atoms occupy crystallographic positions of two different types, with each type constituting a magnetic sublattice. Magnetic structures of a special type, impossible in magnetic crystals, have been discovered in chemically disordered solid solutions (alloys) (see Amorphous magnetic substances, Spin glass, Asperomagnet). A particular form of modulated magnetic structure, the spin density wave whose period may be incommensurable with the crystal lattice period, may appear in a system of delocalized electrons. All the above magnetic structures have been observed in a number of materials, such as those involving 4f -elements and their alloys (see Magnetism of rare-earth metals), as well as actinidecontaining compounds. There is still another form of magnetic structure called the antiphase domain structure which possesses an alternating sequence in space of the groups of n1 atoms with the magnetic moments oriented along a certain axis, and of the groups of n2 = n1 atoms with opposite

magnetic moment orientations (e.g., in thulium, n1 = 4, n2 = 3). ATOMIC ORBITALS See Orbitals. ATOMIC ORDER on a crystal surface

The ordered arrangement of surface atoms (ions, molecules) that corresponds to a minimal free energy (see Thermodynamic potentials) of a ﬁnite crystal. The order is determined by the interaction of surface atoms with one another and with bulk atoms. It can differ from the arrangement in atomic planes inside a crystal, but parallel to the surface (see Surface superlattice, Surface reconstruction). The possible symmetry types of periodic surface structures are described with ﬁve parallelogram systems of equivalent points (twodimensional analog of Bravais lattices, see Twodimensional crystallography) with primitive unit cells in the shape of a general parallelogram, rectangle, square, rhombus with angle 120◦ , rhombus with angle unequal to 120◦ (in this case, one usually chooses a centered rectangle as a nonprimitive cell). Sometimes, the equilibrium state of a crystal surface is in correspondence with the ordered arrangement of vacancies, adsorbed atoms, atomic steps and terraces on it, e.g., a system of equidistant atomic steps of the same height on the facets with high Miller indices (see Crystallographic indices) in silicon and germanium. The results of surface structure studies by scanning tunneling microscopy, and by low-energy electron diffraction, indicate the presence of atomic order on a crystal surface. ATOMIC RADII

The approximate sizes or radii r a of particular atoms in crystals, assuming them to be spheres touching each other. A typical interatomic spacing between two atoms in a crystal is the sum of their atomic radii. In neutral atom crystals such as solid argon the electron density distribution of outer shells of atoms displays a relatively weak dependence on their nearest neighbors. The value of the outer shell radius averaged over the sphere, which characterizes the atomic size, varies with

ATOM–SURFACE INTERACTION

changes in the chemical composition of the nearest neighbors by a few percent when the number of neighbors (referred to as the coordination number k) is the same, and it varies by up to 10–12% in compounds with different coordination numbers. Common coordination numbers are k = 12, 8, 6, and 4 for face centered cubic (fcc), body centered cubic (bcc), simple cubic (sc) and diamond (ZnS) structures, respectively. Thus, an approximate additivity rule exists: d(AB) = r a (A)+r a (B), where d is the closest distance between atoms A and B in the compound AB, and the r a are their atomic radii. In view of the approximate character of the additivity rule, there is some indeterminacy in the choice of numerical values of atomic radii, and several systems of atomic radii exist. All of them, however, predict values of interatomic distances in crystals with a good accuracy, which has been conﬁrmed with many compounds. The metallic atomic radii r M for k = 12, 8, 6, and 4 are in the ratio 1 : 0.98 : 0.96 : 0.88. The atomic radii for Li, K, Al, Fe, Au are 1.55, 2.36, 1.43, 1.26, 1.44 Å. To describe ionic compounds ionic radii r i are used; with the closest distance between two ions of opposite sign assumed to equal the sum of their ionic radii. Underlying the determination of r i are the radii of ﬂuoride (F− ) and oxygen (O2− ), which are adopted to be r i (F− ) = 1.33 Å, r i (O2− ) = 1.32 Å in the Goldschmidt system and r i (F− ) = 1.36 Å, r i (O2− ) = 1.40 Å in the Pauling system. The concept of atomic radii can be extended to other cases. Covalent atomic radii r c are characterized by a noticeable dependence on the bond multiplicity. The value r c for the atoms C, N, O, S reduces by 12–14%, if two pairs of electrons take part in the bond, and by 20–22%, if three, relative to a single electron pair covalent bond. The covalent atomic radii of C, Cl, Br are 0.77, 0.99, 1.14 Å. In molecular crystals, the additivity condition is approximately met for distances d between the nearest atoms of neighboring molecules. One can introduce a system of intermolecular atomic radii r V (also referred to as van der Waals atomic radii). Due to the relative weakness of their bonding forces, the values of r V are greater than those of atomic radii for strong bonding. For He, C, Cl, Kr, r V = 1.40, 1.70, 1.78, 2.02 Å.

91

ATOMIC STEPS on a surface

Raised boundary regions in a monocrystal that are transitions between terraces – ﬂat regions of atomically smooth surface (see Atomically clean surface). The steps are as high as one or several interplanar distances. As distinct from analogous steps of macroscopic size with a height of several micrometers and more, depending on the extent of a surface treatment, the atomic steps cannot be observed with an optical microscope, but are detectable using low-energy electron diffraction and are observable with an electron microscope, a scanning tunneling microscope, or an atomic force microscope. In experiments involving the reﬂection of heavy ions with energy 1–50 keV under grazing incidence on a monocrystal surface with a variation of the angle of incidence, the scattering by the atomic steps “upward” and “downward” (relative to the incident beam direction) produces characteristic features in the energy spectrum of the scattered ions, and marked differences in the extent of their ionization. This allows the use of the scattering of medium energy electrons to diagnose the step structure of a solid surface at the atomic level. ATOMIC STRUCTURE OF A SURFACE See Surface atomic structure. ATOM–SURFACE INTERACTION The interaction of atoms that is deﬁned by

characteristic features of their position on the surface. The crystal surface has an excess of energy compared to the bulk. The coordination number of surface atoms is less than that of the atoms in the bulk (see Coordination sphere), which causes the appearance of uncompensated elastic forces acting on the surface atoms. The formation of a surface can be accompanied also by the appearance of atomic dipole repulsive moments caused by the shift of electron clouds into the depth of a crystal due to the electric potential jump on the surface. The effect of these factors is that the dynamical characteristics of the surface atoms are changed compared to those in the bulk: growth of atomic vibration amplitude, decrease of effective Debye

92

ATTENUATED TOTAL INTERNAL REFLECTION

temperature, and so on. Reconstruction of the upper atomic planes caused by the tendency to reduce the free surface energy, and the phenomenon of a surface phase transition in the absence of one in the bulk (see Atomically clean surface) are typical for a number of crystal surfaces. The screening of the Coulomb interaction of adsorbate atoms by charge carriers in a nearby-surface space charge region can appreciably modify the atom–surface interaction. ATTENUATED TOTAL INTERNAL REFLECTION, ATR method

Technique for studying optical properties of solids (see Optics of solids), based on the phenomenon of total internal re ection of light, which occurs when a light wave penetrates from an optically denser medium 1 into medium 2 of lower optical density (n2 < n1 ). Provided that the angle of incidence ϕ exceeds the critical value ϕcrit = arcsin(n2 /n1 ) there forms a nonuniform (decaying) ﬁeld E(z) = E0 exp(−z/dpenetr ) (z is normal to the interface between the media), with an effective penetration depth dpenetr that is close to the radiation wavelength. Now, assuming that medium 2 is absorbing, the re e ctance is R = 1, which indicates the presence of attenuated total internal reﬂection. The characteristics of spectra recorded by this reﬂection (1 − R) method, and by the standard absorption method, are similar to each other. That is why attenuated total internal reﬂection is used to study strongly absorbing media, and in particular optical properties of their surfaces (e.g., perturbed unstructured layers, adsorption ﬁlms, transition layers of various origins). To enhance the contrast accumulated during repeated internal reﬂections, specially designed prisms are used that provide multiple reﬂections which effectively extend the optical path of the light wave through medium 2. The propagation of light through medium 2 may result in its polarization, so one may speak about the propagation of a volume polariton wave. From the law of the conservation of the tangential component of the wave vector kx it is possible to determine the dispersion of volume polaritons in medium 2: kx = (ω/c)[ε2 (ω)]1/2 where ε2 (ω) is the relevant dielectric constant. If medium 2 appears surface active in the respective frequency range, i.e. ε2 (ω) < 0, one may apply a modiﬁed

type of attenuated total internal reﬂection to excite surface polaritons. To that end, one introduces an air (or vacuum) gap between the prism and the material under study [Otto modiﬁcation (A. Otto, 1968)], or places the material on the base of the prism as a thin ﬁlm [Kretschmann modiﬁcation (E. Kretschmann, 1968)]. ATTO. . .

A decimal preﬁx denoting a 10−18 part of the initial unit of a given physical quantity. For example, 1 as (attoseconds) = 10−18 s (seconds). AUGER EFFECT in semiconductors (P.V. Auger, 1925)

A semiconductor analogue of the Auger effect in an atom; a double electron transition with one electron crossing to a lower level, and another one to a higher level which is often in the continuum, outside the atom. The presence of energy bands of two kinds of current carriers, and the variety of structural defects in semiconductors, leads to the wide diversity of the Auger effect. The role of this effect in nonequilibrium processes in semiconductors may be quite different: recombination, generation, impact ionization of local centers, participation in scattering processes, relaxation of the energy and momentum of charge carriers. This effect can also be a cause of the strength and of the temperature extinction of luminescence. The set of Auger effect variants is shown in Figs. (a–h). There are processes with participation of a multiply charged local center (a), singly charged local center (f, g), two singly charged local centers (b, c, d, h), and free charge carriers (e). Included among Auger processes are also all processes that are inverse to those represented in this ﬁgure. A salient feature of an Auger processes is the pronounced dependence of its probability on the distance R between the interacting carriers (∝ R −6 , corresponding to the energy of one dipole in the ﬁeld of another). In the case of an Auger interaction between free carriers, this means that the rate varies as the square of their concentration. Thus, in process (e), the hole lifetime with respect to the Auger process is proportional to the inverse square of the electron concentration, which means the dependence of the rate on R −6 . Both the theory of the Auger effect and experimental data demonstrate that the probability of this process in semiconductors is weakly

AUGER ELECTRON SPECTROSCOPY

93

Auger effect processes in semiconductors.

dependent on the temperature. The dependence of the probability on the energy exchanged between the carriers is a power function with an exponent between 2 and 5. When the distance between the electrons involved in the Auger interaction mechanism is about 10 nm in order of magnitude (corresponding to a free charge carrier concentration about 1018 cm−3 ), the cross-sections of the Auger processes can be quite large (close in a crystal unit cell size, i.e. ∼10−15 cm2 ). In this case, the Auger processes can dominate the recombination and scattering, thus determining the lifetime of the carriers, the probability of radiative and nonradiative quantum transitions, the relaxation times of energy and momentum, and other parameters of the material. AUGER ELECTRON SPECTROSCOPY

A method of analysis of the elemental and phase composition of surface layers of solids, based on the eld ionization of atoms excited by a beam of primary electrons with energies 1 to 10 keV. The sensitivity of the method is 1010 –1012 atom/cm2 , and the depth of the analyzed layer is 0.5 to 2.5 nm. The mechanism for the emergence of Auger electrons is a complicated multistage process that includes the ionization of an inner atomic level x, the ﬁlling of the produced vacancy by an electron from a higher atomic level y, the nonradiative transfer of the released excess energy to an electron

at level z, and the emission of the Auger electrons. The identiﬁcation of chemical elements is based on comparison of calculated and experimentally found values of Auger electron energy Exy = Ex − Ey − Ez + U eff . Here, Ex , Ey , and Ez are, respectively, the binding energies of electrons at x, y, and z levels (generally designated by X-ray terms) of the neutral atom participating in the Auger process; U eff is a factor to allow for the presence of two vacancies in atomic shells. Auger lines of different elements are well resolved. The change in the electron density at an atom results in a shift of the Auger line, the magnitude and sign of the shift being characteristic of the atom’s chemical state. Analysis of the width and shape of the Auger lines, whose formation is participated in by valence band electrons, yields information on the band structure of a solid. The total Auger electron current is proportional to the number of vacancies at atomic levels formed per unit time within the thickness of the region of the exit from the surface. This circumstance underlies the application of Auger electron spectroscopy to the quantitative analysis of solids. In the scanning mode of the electron beam deﬂection, Auger electron spectroscopy is used for studying the planar distribution of chemical elements with a spatial resolution of a few tens of nanometers. In combination with ion etching, it is applicable for determining the depth proﬁles of element distributions.

94

AUGER ION SPECTROSCOPY

AUGER ION SPECTROSCOPY

Determination of the elemental and chemical composition, the structure, and the state of a solid and its surface from Auger electron spectra (see Auger electron spectroscopy) excited by ion bombardment. An important feature which distinguishes Auger ion spectroscopy from Auger electron spectroscopy is its selectivity, i.e. Auger peaks of a particular kind speciﬁc for a given solid are typically observed in Auger spectra excited by ion bombardment. In addition, these peaks appear only under bombardment by certain ions. In contrast to the electron bombardment case, the character of ion-stimulated spectra is determined by characteristics of the ionization process in the inner shells, and the emission of Auger electrons at atomic collisions. In particular, the ion Auger spectra have a great number of satellites, and represent quasi-molecular spectra with a typical continuous background. Yet many of Auger peaks are narrower, since they are emitted by free atoms dislodged from the solid. Furthermore, the recoil atoms that emerge under ion bombardment and emit the Auger electrons are very fast moving, and induce an extra “Doppler” broadening (see Doppler effect). Under ion bombardment of monocrystals, one can observe both azimuthal and polar orientation effects in the Auger spectra, which are related to the crystal structure of the surface. Also classiﬁed as Auger ion spectroscopy is ion-neutralization spectroscopy that deals with the analysis of the spectrum of secondary electrons emitted during the Auger neutralization of slow positive ions (including multiply charged ones) at the solid surface. Auger ion spectroscopy is a convenient method for diagnostics of the solid surface, and is effective when one has to detect atoms of a certain element or a group of elements on the surface, or during a layer-by-layer analysis of a thin layer. This is particularly convenient in devices where ion beams are used for implantation, etching, spraying, epitaxy, etc. AUGER NEUTRALIZATION

The process whereby an ion near a solid surface traps an electron (or several electrons in the case of multiply charged ions), with subsequent transfer of the resulting energy of neutralization to another (or other) electron(s) in the solid by

means of the Auger process (see Auger effect). A condition for Auger neutralization is that the ionization potential of the ion Vi must exceed the work function of the solid ϕ (Vi > ϕ), and for electron potential emission we require Vi > 2ϕ. The Auger neutralization rate W depends on the scattering of ions to the surface S in accordance with W = A exp(−S/a) where A ∼ 1016 s−1 , a ≈ 0.2 nm. A consequence of intensive Auger neutralization is a low (≈1%) degree of ionization of atoms with high ionization potentials, e.g., inert gases reﬂected from a metal surface. Auger neutralization underlies the ion-neutralization spectroscopy of a solid surface that allows one to determine the electron density in the conduction band, the position of the Fermi level, and other characteristics of the electronic structure of a solid surface. The Auger neutralization of multiply charged ions proceeds stepwise, as a series of successive acts of Auger neutralization and Auger relaxation in the system of levels of ions with decreasing charge, with a mean step of about 25– 30 eV. As a result of the neutralization, the number of emitted Auger electrons is proportional to the resultant energy of the ion neutralization, and can be as high as a few tens of electron volts. On the surface of nonmetals this effect leads to the accumulation of a positive charge (considerably larger than the initial charge) in a microscopic region, and could possibly lead to a Coulomb explosion. This causes sputtering of the solid, and represents a mechanism for metal surface erosion under action of slow multiply charged ions. Auger neutralization of multiply charged ions on the metal surface can serve for their identiﬁcation on the background of singly charged ions due to stimulated electron emission. AUGER RELAXATION Nonradiative relaxation of an excited atom near a solid surface, an analog of the Penning effect in

gases. During Auger relaxation, the excitation energy is transferred by the Auger process to an electron of the solid, which can be emitted outward. Along with Auger neutralization, Auger relaxation is a mechanism of potential emission of electrons. This relaxation is possible for both metastable excited atoms coming to the surface, and ions that trap electrons from the solid at excited levels. The

AUTOIONIZATION

Auger relaxation time is 10−14 to 10−15 s, which is six orders of magnitude less than the time of radiative relaxation. This circumstance suppresses strongly the radiation of the excited atoms near the metal surface. On the surface of nonmetals or metals covered by adsorbed layers, the rate of the Auger relaxation can be slightly smaller. AUGMENTED PLANE WAVES METHOD, APW method (J.C. Slater, 1937) One of the main band structure computation methods. It considers crystal potentials in the form of a muf n-tin potential (MT potential) and is based

on the variational principle. Its basis functions are the APWs. Outside the MT-sphere an APW is a plane wave, ei(k+G)r (G is a reciprocal lattice vector). Inside the MT-sphere the APW method employs a linear combination of solutions of the Schrödinger equation in a spherically symmetric potential. The coefﬁcients for that combination are selected to satisfy the continuity condition for APWs at the MT-sphere boundary. The amount of computations needed follows from the necessity of solving a nonlinear secular equation of high order. The order of the equation, i.e. the number of APWs, is usually quite large, from several dozen for the simplest lattices to several hundred for polyatomic structures. For the linearized APW method, see Linear methods of band structure computation. AUSTENITE (named after W. Roberts of Austen) A high-temperature gamma phase that is a solid solution of carbon (or nickel, manganese, ni-

trogen) in γ -iron with a face-centered cubic lattice (see Face-centered lattice). Alloying with these elements stabilizes γ -iron. Alloys in which the γ -state is present at room temperature are called austenite alloys. They are easily deformable and possess high corrosion resistance. Carbonaceous austenite is stable under cooling to 725 ◦ C; at lower temperatures, a phase transition occurs which can proceed either in a diffusion or a nondiffusion manner, depending on the cooling rate or the isothermal exposure. At cooling rates of a few tens of a deg/s or at isothermal exposure in the temperature range 450–723 ◦ C, the austenite decomposes into a ferrite–cementite mixture (see Cementite) and forms structures of a

95

pearlite class (pearlite, sorbite, troostite) that differ in the degree of dispersion of cementite plates. At temperatures below 450 ◦ C, when the diffusion rate of iron and alloying elements is insufﬁcient, austenite transforms into bainite; the transformation needs only the diffusion of carbon. At lower temperatures and at a cooling rate greater than 100 deg/s, austenite transforms into martensite in a diffusionless manner (see Martensitic transformation). When overheated above the critical point, perlite transforms into austenite at a varying rate; however, the newly formed austenite is heterogeneous even within a single grain volume. To obtain a homogeneous austenite, it is necessary to operate at a temperature above the completion of the perlite–austenite transformation, which produces homogenization. The rate of the homogenization is largely determined by the initial structure of the steel. The trends of the processes of decomposition (see Alloy decomposition) and formation of austenite underlie the processes taking place during the heat treatment of steel, with the treatment providing the required combination of strength and durability properties of steel. AUTOEPITAXY, homoepitaxy

The oriented and ordered build-up of a material on a monocrystal surface of the same material. Autoepitaxy is observed in the deposition of material from liquid solutions or melts, by chemical reactions at crystallization from the gas (vapor) phase, and at condensation from vapors in vacuo. In autoepitaxy the crystal lattice of the building-up phase is oriented relative to the lattice of the substrate monocrystal. Important inﬂuences on autoepitaxy are the chemical purity and the distribution of defects on the monocrystal surface, the chemical composition of the environment, the temperature, the goodness of the vacuum chamber, and the chemical composition of the residual atmosphere. The phenomenon of autoepitaxy is used to prepare thin lms of germanium, silicon, gallium arsenide and other semiconductors on monocrystal substrates of the same materials (see also Epitaxy). AUTOIONIC MICROSCOPY The same as Field ion microscopy. AUTOIONIZATION The same as Field ionization.

96

AUTOPHOTOELECTRONIC EMISSION

AUTOPHOTOELECTRONIC EMISSION

AUTOWAVES

Electronic emission by a conducting body being irradiated by light in the presence of a strong external electric ﬁeld (of the order of 109 V/m). The mechanism of autophotoelectronic emission is the eld electron emission excited by light. This emission appears most prominently in p-type semiconductors at low temperatures. The light excites the electrons from the valence band to the conduction band, with the long wavelength (red) limit of photosensitivity determined by the width of the band gap. The external electric ﬁeld penetrates deeply inside the cathode and facilitates the transport of electrons to the surface and their escape into the vacuum. The quantum yield can reach 0.5–0.8. Autophotoelectronic emission is used in converters of images in infrared rays to visible images. The cathodes in such converters are multitip (up to 106 tips/cm2 ) matrix systems of p-type semiconductors (silicon, germanium, and others).

Nonlinear waves in an active medium, in which the energy dissipation is compensated by an applied external source; the analog of the selfoscillations for distributed oscillatory systems. As distinct from auto-oscillations, when the system oscillates as a whole, in autowave processes the excitation is transferred between neighboring elements of the medium (the term autowaves was introduced by R.V. Khokhlov). There is a great variety of autowave process types in nonequilibrium systems. They are described by systems of non-linear differential equations; a typical form of the equation for the variables Ui , e.g., temperature, particle concentration (quasiparticles in solids), electric ﬁeld, etc., is

AUTORADIOGRAPHY, radioautography

Analysis of the radioactivity distribution in a material by means of autoradiograms which are photographic images produced by radioactive emission. Autoradiography is based on the ability of some substances (typically, silver bromide) to undergo chemical transformations under the action of light, X-rays, gamma rays, and charged particles. Using contact contrast analysis, the emission intensity and the radioactive isotope distribution in the material are determined by the extent, density, and distribution of the blackening of the various regions of the autoradiograms. To obtain and analyze the autoradiogram, a sample containing the radioactive isotope is brought into contact with the photoemulsion and kept in position there for some time (up to several days), depending on the emission type and intensity. Then the autoradiogram is developed and analyzed by means of an optical or electron microscope. In the latter case, the object under study is a carbon replica with emulsion deposited on its surface. Autoradiography is used in the tracer analysis method for studying the distribution of doping elements and impurities in various materials, for measuring their mobilities, etc.

∂Ui = Di ∇ 2 Ui + Fi (U ), ∂t where t is the time, and ∇ 2 is the Laplacian. The ﬁrst term describes the evolution of Ui relative to the spatial spreading of this nonuniformly distributed variable (if Ui is the particle concentration, then Di is the diffusion coef cient, if Ui is the temperature, then Di is the thermal conductivity coefcie nt, etc.). The functions Fi (U ), where U is a totality of the all the individual Ui , describe the non-linearity of the medium, and the interaction between different components of U . These functions include the permanent energy source, which covers the energy dissipation expenditure. There are also more complicated sets of equations describing autowave processes. Self-organization is possible (see Synergism) in autowave media, i.e. the spontaneous regularization of both the temporal evolution of the system (rise of periodic or more complex oscillations) and the spatial distribution of its characteristics (emergence of dissipative structures). However, complete randomization of autowaves often occurs. Autowave processes are widespread in nature, occurring in many biological systems, and in physical and chemical transformations (e.g., combustion and other reactions, gas discharges). In solids, autowave modes are often realized in the excitation of the electron subsystem: in semiconductors by an electric ﬁeld, by heating, by the injection of charge carriers (thermoelectric domains, Gunn effect, recombination waves, electron–hole

AZBEL–KANER RESONANCE

drops, etc.); in phase transitions, e.g., a metal– semiconductor transition, in ferroelectric phase transitions, in active non-linear optical solid media (lasers, real-time holography), etc. The autowave processes in solids are characterized by a variety of spatial–temporal scales (diffusion length 105 –10−7 cm, frequency 10−2 –1010 Hz), and mechanisms of the excitation transfer (ﬂuxes of electrons and holes, excitons, magnons, phonons, photons). Applications of autowaves are extensive, including, for example, optical, radio-, and UHF ampliﬁers and generators; generation of ultra- and hypersound; recording and processing of information; image recognition; processes (propagation of nerve impulses and regimes of cardiac muscle operation), etc. AVALANCHE OF PHONONS See Phonon avalanche.

97

AVOGADRO NUMBER (A. Avogadro, 1811) The number of molecules (atoms, ions) in one mole, identical for any substance in any state of matter; NA = 6.02214·1023 mole−1 . One mole

(gram-molecule) is the mass of a substance in grams, numerically equal to its atomic or molecular weight. The unit of molecular weight is 1/12 of the mass of the carbon isotope 12 C. In the SI system, the mole is accepted as the unit of the quantity of a substance. AXIAL SYMMETRY

The symmetry of a body, which comes into coincidence with itself when rotated through an arbitrary angle about some axis. Such a rotation symmetry axis (∞) pertains to cones and cylinders with the limiting symmetry groups ∞, ∞2, ∞m, ∞ , ∞ m corresponding to them. m m AZBEL–KANER RESONANCE The same as Cyclotron resonance in metals.

This Page Intentionally Left Blank

Bb named after E. Bain. In carbon steels, bainite forms during the isothermal hardening process as a result of decomposition of the austenite (see Alloy decomposition) in the temperature range 250–450 ◦ C. In some alloyed steels (see Alloying), bainite can appear during cooling in air. The conditions of decomposition (mainly, thermal conditions) of the overcooled austenite,determine the formation of higher bainite or lower bainite with speciﬁc morphologic and crystalline features. The transition between them occurs at 350 ◦ C. The bainite structure allows one to process steels that have high static, dynamic and cyclic strength as well as wear resistance and elasticity.

BACKSCATTERING of high-energy particles Occurs under bombardment of a solid surface,

and results from collisions of incoming particles with atoms of the target. In this case the direction of the normal component of the particle momentum may change, which causes some of the particles that have penetrated into the target to escape back through the surface under bombardment. Contributions to backscattering come from both single scattering through large angles, and from multiple scattering. The energy and angular distribution of the scattered particles carry information about the masses of the target atoms; it is the collisions with these atoms in the nearsurface region that determine the energy loss by the incident particles. This effect is used for the analysis of the elemental composition of materials, including their impurities. Ions with energy E 1 keV are almost completely backscattered from most solids. At E 10 keV, a signiﬁcant number of ions penetrates into the target, thus reducing the efﬁciency of the backscattering, especially for heavy ions. The energy of the escaped atoms decreases with increasing depth z where the reversal in direction occurrs, thus allowing an estimate of z. The efﬁciency of the backscattering method for determining the content of defects in crystals (especially impurity and intrinsic interstitial atoms) grows signiﬁcantly for irradiation in the channeling regime. Here, one can determine the positions of interstitial atoms in the channels of a monocrystal target with a good accuracy, and detect the disordering of crystal lattices at a depth of several micrometers from a surface that is irradiated with ions.

BALLISTIC AFTEREFFECT

An inertia effect occurring when a magnetic bubble domain is displaced under the action of a pulse of a nonuniform magnetizing ﬁeld, and continues its motion at the initial speed after the pulse termination. The path covered can be much greater than the domain displacement during the pulse action. The ballistic aftereffect is observable only when the magnetizing ﬁeld gradient along the domain diameter exceeds a certain critical value. The cause of the ballistic aftereffect is as follows: in the overcritical regime, there appears a great number of horizontal and vertical Bloch lines in the magnetic domain wall of the magnetic bubble domain; these lines are dynamically stabilized and accumulate considerable mechanical momentum. After turning off the nonuniform magnetic ﬁeld, the magnetization distribution in the domain wall becomes unstable, and the process of “untwisting” of the Bloch lines begins. The decrease of accumulated mechanical momentum is compensated for by the motion of the domain as a whole. The magnetic bubble domain eventually comes to a stop due to viscous friction forces (see Domain wall drag).

BAINITE, acicular troostite

A structural component of steel, a highly disperse mixture of ferrite and iron carbide. It was 99

100

BALLISTIC PHONONS

BALLISTIC PHONONS

Nonequilibrium acoustic phonons propagating unhindered in crystalline solids, usually in straight line paths without scattering by lattice defects, free current carriers and impurity atoms, and also free of phonon–phonon scattering at low temperatures. A typical distance that phonons of frequency nm (or equivalently κ > 0); where g is the density of electron states at the Fermi surface. The drawbacks of the Stoner model have not yet been completely overcome. One of them is the disregard of the Bloch factor in the wave function of the electrons, the factor having the period of the crystal lattice, which precludes the quantitative treatment of the situation ζ > ε, and thus restricts quantitative results to the case of so-called weak band ferromagnets (κ 1). Another drawback involves the molecular ﬁeld approach that is inapplicable in the neighborhood of the Curie point T C (near point T = T C , B = 0 in the (T , B) plane). Following from Eqs. (1) is the so-called Wohlfarth isotherm (E.P. Wohlfarth, 1968), which is the

102

BAND STRUCTURE

dependence of the magnetization of a band ferromagnet on B and T : m(B, T ) 3 m(B, T ) T2 2χ B − 1− 2 = 0 , m0 m0 m0 TC (2) where m0 ≡ m(0, 0), and χ0 is the longitudinal (in B) static magnetic susceptibility at T = 0. Eq. (2) is quantitatively valid for weak band ferromagnets, e.g., ZrZn2 , ScIn, Ni3 Ga, and a number of Fe–Ni–Mn alloys. The quadratic dependence of the spontaneous magnetization on the temperature, which follows from Eq. (2), viz. m20 − m2 (T ) ∝ T 2 , was also experimentally observed in strong band ferromagnets (3d-metals and alloys). The theory of magnons in band ferromagnets is based on the work of A.A. Abrikosov and I.E. Dzyaloshinskii. The temperature dependence of the magnon spectrum in band ferromagnets was studied by V.P. Silin and others. If the Stoner criterion (1) is not met then the metal is paramagnetic. If, however, |κ| 1, then strong band paramagnetism occurs (for band antiferromagnetism see Antiferromagnetic metals, Spin density wave). BAND STRUCTURE

This is the energy spectrum (plots of average energy E versus wave number k) of singleelectron states represented in the form of a dispersion law of electrons Ekλ , where k is the quasiwave vector, λ is a quantum number called the band index or band number. Occasionally, electronic wave functions are also included in this definition. The band structure is a key notion of the band theory of solids. See also Band structrure computation methods. BAND STRUCTURE COMPUTATION See Linear methods of band structure computation. BAND STRUCTURE COMPUTATION METHODS

Procedures and algorithms for solving the single-particle Schrödinger equation in a periodic potential by using modern computers. The construction of a crystalline potential, self-consistent in the sense of density functional theory, is an

important part of band structure computation. Pseudopotential methods generally incorporate a weak pseudopotential; and full-electron methods place no restrictions on the potential strength. Early band structure computation methods had been developed even before high-speed computers were available. These were the augmented plane waves method (APW), Korringa–Kohn–Rostoker method (KKR), orthogonalized plane waves method (pseudopotential method, version I), and tight binding method. The APW and KKR methods are designed for a potential of a special form. The further development of band structure computation methods was chieﬂy determined by the emergence of linear methods of band structure computation, e.g., linear combination of atomic orbitals (LCAO), linear APW, etc., and generalizations of the methods of the APW and KKR families to potentials of arbitrary form. Standing apart are methods related to the tight binding approach, viz. the linear combination of atomic orbitals method (Gaussian orbitals and Slater orbitals). One can notice their connection to the methods of the KKR theory. The time required for computing the band structure is determined, mainly, by the number of atoms in a unit cell. In most of the methods the computational time grows approximately proportional to the cube of this number. BAND STRUCTURE, SURFACE See Surface band structure. BAND THEORY of solids

A theory describing a crystalline metal or solid as a system of noninteracting electrons, moving in a periodic potential. The potential is assumed to arise from nuclei or positive ions screened by electrons. The effects of mutual interactions are considered to be included in the effective potential. The Bragg scattering of electrons in the crystal potential results in a complicated dependence of electron energies on quasi-momenta (so-called band structure), with the appearance of band gaps, i.e. energy gaps where the electrons have no allowed states. In the ground state, at zero temperature, all electron states with energies lower than the chemical potential (referred to in band theory as the Fermi energy E F , or Fermi level) are occupied,

BAND THEORY

103

Energy bands of (a) the insulator crystalline xenon, (b) the semiconductor silicon, (c) the transition metal molybdenum, and (d) the nearly free electron metal sodium.

and those with higher energies than the chemical potential are empty. In semiconductors and insulators the chemical potential lies within the gap, so there are no allowed states with the energy E F itself. There are such states in a metal, and they form a surface in k -space, called the Fermi surface. An important parameter of the electronic spectrum is the density of electron states, which indicates the number of allowed states per unit energy at a given energy. The density of states at the Fermi level is of special importance. The main task in band theory is to solve the one-electron Schrödinger equation in a crystal potential with translational symmetry. The latter imposes certain constraints on a solution ψk with quasi-momentum k: ψk (r + R) = ψk (r)eikR , where R is a lattice translation period (Bloch theorem). Such solutions are called Bloch wave functions. The requirements of crystal symmetry also impose other constraints on the wave functions and the electron energy spectrum, and these are often used to simplify the solution of the

Schrödinger equation. However, in the vicinity of nuclei the inﬂuence of crystal symmetry is not pronounced, and the potential is close to an atomic one. Hence, it is possible to speak about electronic states (or bands) of predominantly s-, p- or d-type character, similar to the classiﬁcation of states according to the atomic angular momentum. Band theory permits the classiﬁcation of solids according to the qualitative features of their band structure. In insulators the allowed bands do not overlap, and some are completely full (valence bands), while the remainder are empty (conduction bands). Semiconductors differ from insulators only by their small (fraction of an electronvolt) width of the forbidden gap. In metals the Fermi level lies within the allowed band, or more commonly, the allowed bands overlap one another. In semimetals, the overlap of these bands also occurs, but to a lesser extent. There is also a separate class of gapless semiconductors, distinguished by the width of the forbidden gap becoming zero at one or several points of the Brillouin zone.

104

BAND THEORY RELATIVISTIC EFFECTS

Quantitative band theory is based on the numerical solution of the Schrödinger equation in a crystal. Initially used for this purpose were the nearly-free electron approximation and the tight binding method, which are valid within the limits, respectively, of a weak crystal potential, and of a potential consisting of isolated wells separated by high barriers. Later the pseudopotential method was developed, which expanded the applicability of the method of nearly-free electrons. More widely used are non-pseudopotential methods, capable of dealing with more generalized types of crystal potentials. With the appearance of density functional theory, a formal basis emerged for the transformation in the effective potential from a system of strongly interacting electrons to that of noninteracting particles, i.e. to band theory proper. Linear methods of band structure computation have been elaborated, which permit solving the Schrödinger equation in a crystal 2 to 3 orders of magnitude faster than by using classical methods of computation. Typical examples of band structures are shown in Fig. (see previous page): (a) an insulator (crystalline Xe) with a narrow valence band, a wide gap, and bands well described by the tight binding method; (b) a semiconductor (Si) with its indirect gap width small compared to that of the valence band; (c) a transition metal (Mo) with valence electrons comprising the group of bands formed predominantly by s- and d-electrons; where the Fermi level lies inside the d-band with a high density of states; and (d) a simple metal (Na) with s-electrons forming an almost parabolic energy band with a low density of states, in accordance with the model of nearly free electrons, where X, Γ , L, N , and P are symmetry points of the Brillouin zone. BAND THEORY RELATIVISTIC EFFECTS See Relativistic effects in band theory of metals. BAND-TO-BAND TUNNELING See Interband tunneling. BARDEEN BARRIER (J. Bardeen)

A potential barrier which emerges at the boundary between two bodies in contact (e.g., two solids, a solid and a liquid or gas) in the presence of a signiﬁcant concentration of surface electron states at

the interface. In the limit of high concentrations, the Bardeen barrier height does not depend on the contact potential difference due to screening of the Coulomb interaction by the charges in the surface electron state. In practice, the Fermi level of a Bardeen barrier is ﬁxed at the surface (at the interface). In most cases, this term is used with respect to contacts between a semiconductor and a metal (called a Schottky barrier), an insulator, or another semiconductor. BARDEEN–COOPER–SCHRIEFFER THEORY, BCS theory (J. Bardeen, L. Cooper, J. Schrieffer, 1957)

The ﬁrst and the currently accepted microscopic theory of superconductivity based on the presence of so-called Cooper pairs in a superconductor at low temperatures T < T c (where T c is the critical temperature). The Cooper pairs consist of electrons with antiparallel momenta and spins (see Cooper effect) that form as a result of their attraction via the electron–phonon interaction. The starting point of the theory is the model Hamiltonian + 2εk ckσ ckσ + Vkk bk+ bk , (1) HBCS = k,k

k

where εk is the initial energy of the conduction + and ckσ are electrons with momentum k, ckσ the creation and annihilation operators of electrons, respectively, bk+ and bk are the same for the Cooper pairs (see Second quantization), and Vkk are the matrix elements of the effective electron– electron interaction. The minimization of the energy of the ground state of the electron subsystem of the superconductor yields the following expression for the quasi-particle spectrum through the use of the variational method within the BCS framework: 1/2 , (2) Ek = (εk − μ)2 + Δ2k where μ is the chemical potential (Fermi level) of the degenerate electrons in the metal, and Δk is the energy gap determined by the following nonlinear equation: Δ Δ (3) Vkk k tanh k . Δk = − 2E 2k BT k k

A nontrivial solution of Eq. (3) Δk = 0 exists only for the condition Vkk ≡ V < 0, i.e. so in a cer-

BARIUM TITANATE

tain range of energy (momentum) of the Fermi surface of a metal, the effective attraction due to the electron–photon interaction exceeds the screened Coulomb repulsion (see Electric charge screening). In the weak coupling limit Eq. (3) yields the exponential BCS formula for the gap Δ at T = 0: 1 , (4) Δ = 2ωD exp − N(0)V (where ωD is the Debye phonon frequency, and N(0) is the electron density of states on the Fermi surface in a normal metal), and for the critical temperature T c of the transition to the superconducting state we have: 2eγ 1 , (5) Tc = ΘD exp − π N(0)V where ΘD = ωD /k B is the Debye temperature. Eqs. (4) and (5) give the BCS relationship k B T c = eγ Δ0 /π = 0.567Δ0 , where k B is the Boltzmann constant and γ = 0.577. . . is the Euler–Mascheroni constant. The BCS relationship is valid solely for superconductors with weak coupling, whereas for strongly-coupled superconductors k B T c < γ Δ(0)/π . The latter is due to the effects of the retardation of the electron–phonon interaction, which cause the gap Δ to depend on the energy of the quasi-particles and, hence, the value of Δ at T = 0 increases compared to the value πk B T c /eγ . The BCS theory has explained the principal physical properties of superconductors in terms of the presence of the energy gap in the quasi-particle spectrum. This includes magnetic vortices, ﬂux quantization, the exponential dependence of the electron speci c heat on the temperature and its jump in value at the phase transition point T = T c ; the temperature dependence of the thermodynamic critical magnetic eld; the features of ultrasound attenuation; relaxation of nuclear spins, and the absorption of electromagnetic waves in superconductors; the current–voltage characteristics of the superconducting tunnel junctions, and so on. The originators of the BCS theory received the Nobel prize in 1972. BARIUM, Ba

A chemical element of Group II of the periodic system with atomic number 56 and atomic mass 137.33. It consists of a mixture of seven sta-

105

ble isotopes, with 138 Ba predominating (71.66%). The electronic conﬁguration of the outer shell is 6s 2 . Successive ionization energies are 5.21 and 10.00 eV. Atomic radius is 0.221; ionic radius of Ba2+ is 0.134 nm. Oxidation state is +2. Electronegativity is ≈0.94. In a free form barium is a silvery-white soft metal. It has a body-centered cubic lattice with parameter a = 0.5019 nm at ¯ (O 9 ). room temperature; Space group is I m3m h 3 Density is 3.76 g/cm ; T melting = 998 K; heat of melting is 7.66 kJ/mole; heat of sublimation is 205 kJ/mole; T boiling = 1912 K; heat of evaporation is 175 kJ/mole; speciﬁc heat is 284.7 kJ·kg−1 ·K−1 ; Debye temperature is 110 K; coefﬁcient of linear thermal expansion is ≈19.5·10−6 K−1 (at 273 to 373 K); adiabatic bulk modulus is 9.575 GPa; Young’s modulus is 15.57 GPa; rigidity is 6.33 GPa; Poisson ratio is 0.229 (at 293 K); Brinell hardness 0.042 GPa; Mohs hardness is 2; ion-plasma frequency is 4.52 THz, Sommerfeld linear electronic speciﬁc heat coefﬁcient γ is 2.72 mJ·mole−1 ·K−2 ; electric resistivity is 357 n·m (at 293 K); temperature coefﬁcient of the electrical resistance is 0.00649 K−1 ; work function of a polycrystal is 2.49 eV; molar magnetic susceptibility is 20.4·10−6 cgs units; nuclear magnetic moment of 137 Ba is 0.931 nuclear magnetons. Barium is used in alloys with lead, aluminum, and magnesium. Barium and its compounds are added to the materials intended for protection against radioactive and X-ray radiation. BARIUM TITANATE, BaTiO3

A colorless solid substance; T melting ∼ 1618 K; it has the structure of perovskite (tetragonal crystal lattice with lattice constants a = 0.3992 nm, c = 0.4036 nm); density is 6.08 g/cm3 . Each titanium is surrounded by a somewhat distorted octahedron of oxygens. Chemically it is very resistant: it does not change in air or react with water, diluted acids or alkali; it dissolves in hot strong sulfuric acid. It is an insulator with a very high dielectric constant (1000 at 20 ◦ C), and one of the most important ferroelectrics with a high piezoelectric modulus (see Piezoelectricity) and speciﬁc optical properties. It is obtained by caking and melting together of titanium dioxide with barium oxide, hydroxide or carbonate, or

106

BARKHAUSEN EFFECT

by heating up to 800 to 1200 ◦ C of mixture obtained by common deposition of carbonates or oxalates from solutions. It is used in the form of monocrystals and solid solutions for manufacturing of capacitors, piezoelectric cells, pyroelectric collectors of radioactive energy, etc. BARKHAUSEN EFFECT (H.G. Barkhausen, 1919) A jump-like change of magnetization M in

magnetically ordered materials under continuous variation of external conditions (e.g., applied magnetic ﬁeld B). Barkhausen discovered that clicks could be heard in a telephone supplied by an electron ampliﬁer and connected with a coil containing a ferromagnetic sample during very slow (quasi-static) magnetizing of the latter. The main cause of a Barkhausen effect is the various inhomogeneities of the crystalline structure of a ferromagnet (inclusions, residual stresses, dislocations, grain boundaries, the heterogeneity of the composition, and other defects in the crystals). When moving in the magnetic ﬁeld, the magnetic domain walls attach to these inhomogeneities until the increasing ﬁeld reaches a certain (critical) value. Then the domain wall is released (Barkhausen jump), so that its motion turns out to be jump-like, in contrast to a smooth movement in a perfect crystal. These jump-like changes are irreversible. Another mechanism of the Barkhausen effect is possible: the nucleation of new phase centers with their subsequent growth. The Barkhausen effect is best observable in soft magnetical materials at the steepest part of the magnetization curve (of stepped shape in that region, see Fig.). This effect

is highly sensitive to various external factors and structural changes in the sample. The connection of the Barkhausen effect with the magnetic domain structure, the main elements and the shape of the hysteresis loop, allows it to be used as a method of investigation of the domain structure of ferromagnets. By analogy with ferromagnets, the appearance of repolarization jumps in ferroelectric crystals under variation of an applied electric ﬁeld is also referred to as a Barkhausen effect. BARKHAUSEN NOISE

Irregular sequences of jumps in the the magnetic moment of a ferromagnetic sample placed in a periodically varying magnetic ﬁeld (see Barkhausen effect). The component is due to ﬂuctuations of speciﬁc parameters of Barkhausen jumps (the shape and duration, the critical ﬁeld, the magnetic moment varying at the jump, the number of jumps in a given range). Studies of Barkhausen noise yield substantial information on complicated phenomena involving the rearrangement of the magnetic domain structure in ferromagnets. BARNETT EFFECT (S. Barnett, 1909) Magnetizing of ferromagnets under a change in

their mechanical moment. Barnett conﬁrmed Ampère’s hypothesis that magnetism can arise from rotational motion of charges in a material (molecular current hypothesis). In a body with no atomic magnetic structure, the intrinsic magnetic moment is proportional to the angular velocity and oriented along the rotation axis. In some cases, the Barnett effect allows one to determine the gyromagnetic ratio or Landé g -factor of atoms of some materials. In particular, this ratio for Fe, Co, Ni and their alloys corresponds to the electron magnetic moment and indicates that ferromagnetism is mainly due to the electron spin. The Barnett effect, along with the converse Einstein–de Haas effect, are called magnetomechanical phenomena. Magnetic resonance methods are much more precise for determining g-factors. BARODIFFUSIONAL EFFECT An effect of hydrostatic pressure on the diffusion healing of defects, or the retardation of pore

Barkhausen effect.

growth (at low pressures), and on the decrease of

BARRIER INJECTION TRANSIT TIME DIODE

the diffusion coef cient in crystals (at high pressures). At low pressures, barodiffusional effects are caused by the inﬂuence of pressure on the equilibrium between the pore and the vacancy subsystem (see Vacancy) taking into account oversaturation Δ = cv − cv0 in a crystal (where cv and cv0 are the actual and equilibrium concentrations of vacancies, respectively). Under the characteristic pressure Pk = 2α/R0k (where α is the surface tension, R0k is the critical radius of a viable pore embryo in the absence of pressure), the nucleation and the growth of pores are forbidden. At R0k = 10−5 cm, Pk ≈ 102 atm. Such pressure has a signiﬁcant effect on the kinetics of the diffusional coalescence of the pore ensemble due to the transformation of some of the growing pores into dissolving ones. Under high pressures, the barodiffusional effect is caused by the decrease of cv and by the increase of the energy outlay for an elementary migration event with growing pressure. There is an exponential diffusion coefﬁcient dependence ω P , DP = DP 0 exp − A kBT where ωA = ωv + ωm is the activation volume, ωv < ω is the vacancy volume dependent on the extent of relaxation of the atoms surrounding the vacancy, ω is the atomic volume, ωm is the volume of the activated complex at a crossing point between two neighboring positions. It follows from the dependence DP (P ) that at a characteristic pressure P ∗ = k B T /ωA the value of DP reduces e times. For metals, P ∗ ≈ 104 atm. BARRETT FORMULA (J.H. Barrett)

An expression describing the temperature dependence of the dielectric constant of ferroelectrics in the paraelectric phase in a temperature (T ) range that includes the quantum region: ε(T ) − ε∞ −1 Ω0 Ω0 =C , −Tc coth 2k B 2k B T where Ω0 is the frequency of zero-point vibrations, T c is the “high-temperature” value of the Curie–Weiss temperature. At T > Ω0 /k B , the

107

Barrett formula transforms into the classical expression since ε(T ) satisﬁes the Curie–Weiss law. The system behavior at T Ω0 /k B depends on the ratio of T c and Ω0 /(2k B ). If T c > Ω0 /(2k B ), the system has a low-temperature phase transition at T = T cL < T c . There is no ferroelectric phase transition, if T c < Ω0 /(2k B ), in this case the crystal is a virtual ferroelectric. The Barrett formula is used to explain the observed low-temperature values ε(T ) in SrTiO3 and KTaO3 , but is only valid when the soft mode frequency is high relative to acoustical frequencies. In the general case, taking into account the interaction of optical vibrations and acoustic vibrations results in a characteristic modiﬁcation of the Barrett formula in a low-temperature range. BARRIER See Bardeen barrier, Lomer–Cottrell barrier, Potential barrier, Schottky barrier, Local barriers, Surface barrier, Surface barrier structures. BARRIER CAPACITANCE, junction capacitance

Electric capacitance caused by the existence of a potential barrier in a semiconductor junction, in a heterojunction, at a metal–semiconductor junction, and so on. Such a system possesses a high-ohmic layer that is depleted of current carriers and situated between high-conduction layers, i.e. is similar to a capacitor. The electric charge in the depletion layer is concentrated at local electronic levels. The barrier capacitance value is determined by the thickness of the depletion layer and the dielectric constant of the crystal. A layer with an increased current carrier concentration also has a barrier capacitance, e.g., an accumulation layer in the metal– insulator–semiconductor structure. BARRIER INJECTION TRANSIT TIME DIODE (BARRITT diode) A superhigh-frequency (SHF) semiconductor diode consisting of a semiconductor plate with contacts made of semiconductor junctions

(p+ –n–p+ , p+ –n1 –n2 –p+ , where n1 > n2 , and other structures), Schottky barriers (m–n–m structures, m is metal), or their combinations. With the bias voltage applied to the diode, one contact operates in the forward direction and the other in the reverse direction. A BARRITT diode operates in a

108

BARRITT DIODE

punch-through mode where the depletion regions of the forward- and reverse-biased contacts overlap, so that a small change of the voltage across the diode results in the current growing by several orders of magnitude. Dynamic negative resistance in the BARRITT diode arises in a frequency range ω where the phase delay of carrier transit through the depletion layer of the reversebias junction is θ = ωτ ≈ 3π/2 (τ is carrier transit time). The barrier drift time through the depletion layer of the reverse biased junction depends on the width of the depletion layer and the saturation velocity. The effect is due to the phase shift between the SHF electric ﬁeld and the conduction current. The required phase shift is caused: (i) by the phase delay of the injection of the minority charge carriers through the forward biased p–n junction, and (ii) by the ﬁnite time of the current carrier drift through the depletion layer. BARRITT diodes are used for signal generation and ampliﬁcation in the frequency range from 3 to 15 GHz. The main advantage of these diodes is a low noise level. BARRITT DIODE The same as Barrier injection transit time diode. BASAL PLANE of crystals

A plane containing equivalent crystallographic (coordinate) axes x and y. Ordinarily it is the plane that forms the bottom of the conventional unit cell, with the index (001) in tetragonal and (0001) in trigonal and hexagonal crystals (see Crystallographic system). The spatial arrangement of the faces and the sides of crystalline polyhedra is described with the help of symbols relative to these axes. The faces that intersect only one axis and possess numbers (100), (010) and (001) (see Crystallographic indices) are called basal (coordinate) faces. BASALT

An extrusive and congealed dark gray or black volcanic rock consisting mainly of plagioclase, pyroxenes and often olivine, typically with an admixture of magnetite or ilmenite. Color is dark sulfur-like to black. Basalt forms frequently have a rod-like or a “pencil”-like separation. Holocrystalline basalt is called dolerite; basalt of vitreous texture is called hyalobasalt.

The almond-shaped basalts, or mandelstones, are porous varieties. The pores (voids) are of a rounded, ellipsoidal, more rarely elongated, tubular shape and are ﬁlled with minerals, mostly, agate, chalcedony, opal, quartz, or sometimes, amethyst, zeolites, calcite, and so on. The density is 2.8–3.2 g/cm3 ; the resistance to compression in a dry state is 300–500 kg/cm2 (3–5 MPa); electric resistivity ρ = 103 –105 ·m; porosity is 7.9%, water absorption is 1.07%, and magnetic susceptibility χ = (125–15500)·106 CGS units. The basalts are used as building, electric insulation, and acid-resistant materials. BAUSCHINGER EFFECT (J. Bauschinger, 1886) A partial dehardening of single and polycrys-

talline solids observable at the change in the sign of the strain. The effect manifests itself as a reduction of some initial mechanical properties (elastic limit, yield limit, and so on) when, prior to a test, a sample was loaded in the opposite direction until an insigniﬁcant residual strain appears. The Bauschinger effect is observable both in static tests and in the course of fatigue loading (see Fatigue). At the same time, its value depends essentially on the kind of material, of the material pretreatment, and the strain conditions. Numerous attempts have been made to explain the Bauschinger effect on the basis of dislocation theory (see Dislocations); however, a satisfying agreement with the experimental data has been achieved only in individual cases. BEER–LAMBERT LAW (also called Bouguer–Lambert–Beer law, P. Bouguer, J.H. Lambert, A. Beer)

A law determining the dependence of the intensity I of a parallel monochromatic light beam on the thickness d of the absorbing matter: I = I0 e−kd ,

(1)

where I0 is the incident light intensity, k is the absorption coef cient (cm−1 or m−1 ). The latter is related to the dimensionless absorption index κ as k = 4πκ/λ, where λ is the wavelength. Eq. (1) is used to evaluate the absorptivity of a solid or liquid layer. For a dilute solid or liquid solution of concentration n, Eq. (1) takes the form: I = I0 e−χnd ,

(2)

BERYLLIUM

where χ is the molecular absorption index, cm2 . In the particle beam radiation of solids the term absorption cross-section is often employed for χ , and k is referred to as the absorption factor. Sometimes the Beer–Lambert law is expressed in terms of common logarithms (i.e. a power of 10) as I = I0 · 10−εcd ,

(3)

where c is the molar concentration, and ε is the decimal molar absorption index, also called the absorption or extinction coefﬁcient. BEILBY LAYER (G.T. Beilby, 1901) A glass-like surface layer that appears during mechanical processing (grinding, polishing, forging, punching, cutting, and so on) at the surface and over the grain boundaries of crystalline solids (metals, quartz, various minerals and chem-

ical compounds). A Beilby layer has its normal crystal structure obliterated. Long term grinding or polishing is unable to remove the layer, but rather causes its thickness to grow. A Beilby layer is removable by chemical methods. Its thickness ranges from a several to 100 or more microns. A Beilby layer along grain boundaries imparts great strength to a material, it is characterized by pronounced hardness, and speciﬁc optical, electric, and magnetic properties. A Beilby layer crystallizes under heating at a temperature between 0.4 and 0.6 that of the melting temperature. BENDING VIBRATIONS of a crystal lattice Vibrations of chains (layers) of crystal atoms

in a direction normal to the chains (layers). Bending vibrations exist in those crystals where the bonding between the chains (layers) is weak compared to that of the atoms within the chain (layer). The linear dispersion law for bending vibrations is valid only for the lowest values of the wave vector along the chain (layer). At large values of the wave vector, a quadratic dispersion law similar to that for the vibrations of strings and membranes applies. BERKELIUM, Bk An actinide element of Group III of the peri-

odic system with atomic number 97 and atomic mass 247.07.

109

There are 11 known radioactive isotopes with mass numbers 240, 242 to 251 (no stable isotopes have been discovered). Electronic conﬁguration of outer shells is 5f 7 6d 2 7s 2 . Ionization energy is 6.30 eV; atomic radius is 0.174 nm; radius of Bk3+ ion is 0.0955 nm, of Bk4+ ion is 0.0870 nm. Oxidation state is +3 (most stable in solution) and +4 (strong oxidizer). Electronegativity is 1.2. In a free form, berkelium is a silvery-white metal. Stable at a temperature below ∼1250 K is α-Bk with double hexagonal close-packed structure (hexagonal layers alternate 4 ), basic ABAC. . . ; space group P 63 /mmc (D6h parameters a = 0.3416 nm, c = 1.1069 nm at room temperature). Stable above ∼1250 K up to T melting ≈ 1290 K is β-Bk with hexagonal closepacked structure (space group F m3m, Oh5 ; parameter a = 0.4997 nm at room temperature after hardening). Density is 14.80 g/cm3 ; T boiling is about 2880 K. At low temperatures, α-Bk becomes antiferromagnetic with Néel point T N ≈ 22 to 34 K). In β-Bk, no magnetic ordering has been detected. Berkelium isotopes are used for research in nuclear physics and radiochemistry. Berkelium is highly toxic. BERNAL’S FLUID MODEL See Random close-packing model. BERYLLIUM, Be

A chemical element of Group II of the periodic system with atomic number 4 and atomic mass 9.01218. Natural beryllium consists of the stable isotope 9 Be with electronic conﬁguration 1s 2 2s 2 . The ionization energies are 9.323 or 18.21 eV. Atomic radius is 0.113 nm, Be2+ ion radius is 0.035 nm. It is chemically active; oxidation state is +2. Electronegativity is 1.47. In a free form, beryllium is a light bright gray metal, which is brittle under normal conditions. The properties of beryllium depend on its purity, grain size, texture and degree of anisotropy that depend on its pretreatment. Some properties change with an increase of pressure and temperature, and upon strong neutron irradiation (>1023 neutrons/m2 ). Beryllium crystallizes in two allotropic modiﬁcations. Below 1527 K, α-Be is stable (hexa-

110

BERYLLIUM ALLOYS

gonal close-packed lattice with parameters a = 0.2283 nm, c = 0.3584 nm at 300 K and impurity content no more than 1%; space group P 63 /mmc, 4 ). Above 1527 K up to T D6h melting = 1560 K, β-Be is stable (body-centered cubic with parameter a = 0.2546 nm at 1527 K; space group I m3m, Oh9 ). Bond energy of pure beryllium is 3.33 eV/atom at 0 K; density is 1.848 g/cm3 (at 293 K); melting heat is 11.7 kJ/mole; sublimation heat is 314 kJ/mole; T boiling = 2743 K; evaporation heat is 309 kJ/mole; speciﬁc heat is 1.80 kJ·kg−1 ·K−1 ; Debye temperature is 1160 K. Coefﬁcient of linear thermal expansion is 9.2·10−6 K−1 along the principal axis 6 and 12.4·10−6 K−1 perpendicular to it (at 300 K). Heat conductivity reduces from 230 W·m−1 ·K−1 to 178 W·m−1 ·K−1 in the temperature range 273 to 323 K; adiabatic coefﬁcients of elastic rigidity of α-Be monocrystal: c11 = 288.8, c12 = 20.1, c13 = 4.7, c33 = 354.2, c44 = 154.9 GPa at 298 K (within the range 423 to 1530 K c13 0 GPa). Bulk modulus is ≈109 GPa, Young’s modulus is ≈304 GPa, rigidity is ≈143 GPa; Poisson ratio is ≈0.056 (at 298 K); ultimate tensile strength is 0.196 to 0.539 GPa; relative elongation is 0.2 to 2%. Pressure treatment considerably improves mechanical properties; ultimate strength in stretching direction reaches 0.392 to 0.784 GPa; yield limit is 0.245 to 0.588 GPa; and relative elongation up to 4 to 12%; mechanical properties perpendicular to stretching undergo minimal change. Brinell microhardness is 1.18 GPa; impact strength is 0.001 to 0.005 GPa; transition temperature of commercially pure beryllium from brittle to plastic state is 473 to 673 K. Highly pure beryllium (above 99.9%) with grain size 90◦ (see also Uniaxial crystals). BICRITICAL POINT

A point on the phase diagram of a crystal where two curves of second-order phase transitions and one curve of a rst-order phase transition meet. The latter curve usually separates the regions of existence of two different ordered phases (see Multicritical point). BIEXCITON, exciton molecule A bound state of two excitons in semiconductors and insulators.

A biexciton in a semiconductor is a stable fourparticle complex containing two electrons and two holes. Since the effective masses of an electron me and a hole mh in semiconductors are close to each other, the biexciton stability problem has no small parameter for carrying out a power series expansion. Therefore, the adiabatic approximation widely used in molecular spectroscopy is inapplicable in this case; and the calculations are usually carried out with the help of the variational method. In the limit me /mh = 1, the biexciton stability problem is analogous to the positronium molecule problem. The binding energy of the positronium molecule is extremely small: M ≈ 0.02Ex where Ex is the binding energy of the positronium atom (electron–positron bound state analogous to hydrogen atom). For example, the biexciton binding energy in Ge and Si is ΔM 1 meV. Variational calculations of this

BIOLOGICAL CRYSTALS

binding energy in semiconductors with different energy band structures demonstrate that biexcitons are stable for arbitrary values of the ratio me /mh . In the limit me /mh → 0, corresponding to a hydrogen molecule, ΔM = 0.35Ex . Since the energy gain due to biexciton formation from two excitons is insigniﬁcant, from the thermodynamic viewpoint biexciton formation is likely only at low enough temperatures. The probability of formation is in proportion to the square of the exciton concentration; and the estimates show that this concentration should be very large. The most direct method for the detection and investigation of biexcitons is the analysis of their recombination emission spectra. The most probable process of radiative biexciton decay is via a single electron–hole pair recombination accompanied by the creation of a photon and a recoil exciton. The radiative decay of biexcitons was detected in the indirect-gap semiconductors Ge and Si. In direct-gap semiconductors, the recombination times are extremely short (10−9 s or less). Hence, the processes of binding excitons into biexcitons and the nonradiative decay of the latter takes place under highly nonequilibrium conditions with respect to both the phonon system and between the electron–hole components of the system itself. Therefore, to study the biexciton properties in direct-gap crystals experimentally, nonlinear optical methods were developed that are most efﬁcient under highly nonequilibrium conditions. The methods include the two-phonon resonance excitation of biexcitons, the induced one-phonon transformation of an exciton into a biexciton, as well as the two-phonon resonance Raman scattering of light (or hyper-Raman scattering) with participation of biexciton states. The efﬁciency of these processes in direct-gap semiconductors is associated with a very large value of the nonlinear susceptibility at two-phonon resonance in the biexciton state. This is the basis for nonlinear effects of the multiwave mixing (see Frequency mixing) and bistability with participation of biexcitons. With the help of these methods, biexcitons were detected and studied in a number of direct-gap semiconductors (CuCl, CuBr, CdS, etc.).

113

BIMETALS, bimetallic materials

Materials consisting of two different, tightly bonded metals or alloys. A distinctive feature of bimetals is a combination of various properties such as strength and thermal-environment resistance, wear resistance, or low electric resistance. Joining of bi- or multilayer metals occurs via the action of interatomic forces which bring the pure metal surfaces to a separation close to an interatomic one. The bimetals are obtained either using plastic deformation (rolling, pressing, pressure welding, drawing, diffusion welding) or without it (casting, electroslag welding, metallization by spraying, and so on). In industry, bimetals are used for preserving expensive metals or alloys, as well as materials with special properties. Bimetals containing metals (alloys) with different thermal expansion coefﬁcients are called thermobimetals. BINARY ALLOYS, double alloys Alloys formed from two component systems. Binary alloys are used when studying phase diagrams of the phase equilibrium and the phys-

ical, chemical, thermodynamic and other properties of alloys composed of two components. For example, binary alloys of the iron–carbon system, binary alloys based on nickel, and so on. These alloys include single-phase alloys and two-phase alloys, intermetallic compounds, interstitial alloys, and substitutional alloys, as well as various metallic materials regardless of the mode of their manufacture. A common feature is their two-component composition. For two-component alloys (differing in concentration) the term binary alloy system is used (e.g., the melt diagram of the binary system Al–Si). Alloys containing three or four components are called tri-component alloys and tetracomponent alloys, respectively. Alloys composed of four and more components are called multicomponent alloys. BIOLOGICAL CRYSTALS Crystals built of biological molecules (pro-

teins, nucleic acids or virus particles). Due to the enormous dimensions of biological macromolecules containing 103 –104 atoms, biological crystals have very large crystal lattice periods (5–20 nm) compared to ordinary crystals,

114

BIPHONON

Packing of molecules in a protein crystal.

the lattice periods in a virus reaching 100 nm or more. An important feature of biological crystals is that they contain, in addition to the macromolecules themselves, some of the host solution (35–80%), from which the molecules were crystallized, typically water with various ions (see Fig.). Many biological crystals exist solely in equilibrium with such solutions. Desiccation brings about the denaturation (structural decay) of molecules and the crystal as a whole. Regularity of the arrangement of molecules in biological crystals is determined by the electrostatic interaction of the charged atomic groups at the surface of the molecules, with van der Waals forces and hydrogen bonding playing a major role. The solvent molecules adjacent to the surface are arranged in order; those in the intermolecular space are disordered. The methods of crystallization of biological crystals are based on the variation of the temperature and oversaturation. To change the solubility, some particular salts, or organic solutes, etc., are introduced into the solution. The enormous dimensions of biological crystals allow one to directly observe their packing in the crystal lattice with the help of electron microscopy. X-ray diffraction also provides data on the most complicated spatial conﬁguration of the molecules composing the crystals, but the enormous number of reﬂections obtained (100,000) render the process of decoding them extremely complex. In addition to the true three-dimensional periodic biological crystals, there exist biological crystals with different types of ordering. Thus, deoxyribonucleic acid (DNA) forms textured gels, i.e. liquid crystals. Their X-ray structural analysis

allowed a spatial model of DNA to be constructed, and the nature of the genetic information transfer to be established. Some globular proteins (catalase and others) crystallize with the formation of tubes with monomeric walls built of molecules arranged according to spiral symmetry. Research of crystals of spherical viruses with the help of electron microscopy and X-ray analysis allowed one to establish the character of the mutual packing, and the structure of the protein molecules composing the virus shell. The latter are arranged in a virus particle according to icosahedral symmetry, with an axis of 5th order (see Crystal symmetry). BIPHONON A quasi-particle representing a bound state of two phonons, arising due to the anharmonic vibrations.

Both phonons move in the crystal as an integral whole, and are characterized by the same value of the wave vector. A biphonon inﬂuences phonon optical spectra of absorption and spectra of Raman scattering of light as a sharp maximum situated at an energy below the lower edge of the corresponding two-phonon band. The latter characterizes the crystal excitation region for the simultaneous creation of two phonons (the socalled sum process), or at the creation of a phonon of higher energy with simultaneous destruction of another one of lower energy (the so-called difference process). The separation of a biphonon peak from the two-phonon band and its intensity are determined by constants characterizing the anharmonicity, and by the density distribution of twophonon states. Biphonons are frequently observable in phonon spectra at low temperatures. BIPOLAR DIFFUSION The same as Ambipolar diffusion. BIPOLARON

A system consisting of two conduction electrons bound by a strong interaction with the medium; in other words, two bound polarons. The appearance of bipolarons is possible in crystals, amorphous materials, and liquids. If the macroscopic polarization dominates the interaction with the medium then the large dielectric constant of the medium favors the creation of bipolarons. The electron motion in a bipolaron is correlated; an essential feature is their space separation

BIPOLAR TRANSISTOR

inside the polarization potential well. The possibility of forming bipolarons was ﬁrst established analytically in ionic crystals and then extended to amorphous insulators, metals and other materials. In bipolarons the electrons with opposite spins are bound, which leads to the absence of paramagnetism of the free charge carriers. The experimental evidence of the existence of bipolarons was obtained in a series of oxide crystals with variable valence (e.g., Ti4 O7 ), and in some compounds of linear organic molecules. The space–time properties and energy scale of a bipolaron are essentially different from those in a Cooper pair. See also Bipolaron mechanism of superconductivity. BIPOLARON MECHANISM OF SUPERCONDUCTIVITY

A possible mechanism to explain supercurrent ﬂow through a crystal without resistance at low temperatures due to the super uidity of a charged Bose gas or a Bose u id of bipolarons. The elementary excitation spectrum in such a system of charged bosons possesses, due to the long-range Coulomb repulsion, a ﬁnite energy gap E0 = ωp at zero momentum (where ωp is the frequency of the collective plasma oscillations in the bipolaron gas). This also satisﬁes the Landau super uidity criterion, which in this case corresponds to superconductivity. The bipolaron mechanism of superconductivity differs from the Cooper pairing of the Bardeen–Cooper–Schrieffer theory (BCS) in that bipolarons of small and intermediate radii are separated in space, and are not expected to decay above the transition from the superconducting to the normal state. To estimate the critical temperature of such a transition, one can use the expression for the Bose–Einstein condensation tem2/3 perature T0 = 3.312 n0 /m∗B (where n0 is the

115

concentration and m∗B is the effective mass of the bipolarons) of an almost ideal charged Bose gas 1/3 ∗ >1 of high density under the condition n0 aB ∗ = ε 2 /(4e2 m∗ ) is the effective Bohr (where aB 0 B radius of a bipolaron with charge of 2e, and ε0 is the static dielectric constant of the crystal). An estimate T0 2–50 K was obtained for bipolarons of intermediate radius in ionic crystals with ε0 1 of SrTiO3 type at m∗B 10m0 (m0 is free electron mass) and n0 ≈ 1017 –1020 cm−3 , while T0 8–80 K for bipolarons of small radius with m∗B ≈ (100–1000)m0 at n0 1022 cm−3 . The bipolaron mechanism of superconductivity has been proposed theoretically for heavy fermions (CeCu2 Si2 , UBe13 , UPt3 ), semiconducting perovskites BaPb1−x Bix O3 and possibly the new high-temperature superconductor cuprates. BIPOLAR TRANSISTOR A semiconductor device with its active zone containing two semiconductor junctions separated

by a thin region called a base. The outer zones having the same conduction type are called the emitter and collector (see Fig.). In an n–p–n type transistor the minority current carriers of the base (electrons) diffuse through the p-type base region and penetrate the n-type collector region; in a p–n–p type bipolar transistor the minority current carriers (holes) diffuse through the n-type base region. A bipolar transistor is designed in such a way that small variations of the electric current or voltage could cause signiﬁcant current variations between the emitter and the collector. As to their design, bipolar transistors can be either homostructural, heterostructural, or have graded bands. Bipolar transistors serve for the generation and ampliﬁcation of electromagnetic oscillations, and for the control of voltage and current.

Structure (left) and energy diagram (right) of an n–p–n bipolar transistor showing the emitter (e), base (b) and collector (c) regions. The donor and acceptor energy levels are indicated by dashed horizontal lines.

116

BIRADICAL

BIRADICAL

A molecule containing two spatially separated radical centers (unpaired electrons), with the singlet–triplet energy splitting of the orbital state lower than or close to k B T . The appearance of biradicals in a solid causes changes in an electron paramagnetic resonance spectrum due to exchange interactions and dipole–dipole interactions. In chemical reactions, a biradical behaves as two independent, but joined together, free radicals. BIREFRINGENCE Refraction of light in anisotropic media (e.g., crystals), which results in its splitting into two

beams with different polarizations. It was discovered by E. Bartholin (1669) in calcite crystals. Birefringence is caused by the tensorial dependence of the polarization vector of the anisotropic medium on the light wave electric ﬁeld intensity. The result is that the polarization of light in the medium and the phase velocities of the waves (refractive indices) both depend on the direction of propagation. In optically inactive crystals, upon birefringence the two waves are locally polarized in mutually perpendicular planes (in the general case of an optically active crystal the waves are elliptically polarized) and they have different phase velocities. In single-optical-axis crystals one of the waves (ordinary ray) is polarized perpendicular to the main cross-section, i.e. the planes which pass through the direction of the light wave and the optical axis of a crystal, and the other wave (extraordinary ray) is polarized parallel to it. Refraction of the ordinary wave is similar to refraction (see Refraction of light) in an isotropic medium since the ray vector coincides with the wave vector and the refraction index does not depend on the direction of propagation. For the extraordinary wave the common law of refraction is not satisﬁed: the wave and ray vectors do not coincide, and the refraction index n0 depends on the direction of propagation. For light propagation along the optical axis there is no birefringence. Biaxial crystals are characterized by three refraction indices, and they have two directions (two optical axes), along which there is no birefringence. The phase velocities of both waves depend on the direction of propagation, and both waves, upon refraction, may emerge from the plane of incidence.

Birefringence is possible not only in naturally anisotropic media, but also in media with an induced anisotropy caused by external ﬁelds: electrical (Pockels effect, Kerr effect), magnetic (Voigt effect), and acoustical. Phenomena similar to birefringence have also been observed outside the optical range of the electromagnetic spectrum. See also Self-induced light polarization change. BISMUTH (Lat. Bismuthum), Bi

Chemical element of Group V of the periodic table; atomic number 83, atomic mass 208.98. Natural bismuth consists of one stable isotope 209 Bi. Electronic conﬁguration of outer shells is 6s 2 6p3 . Ionization energies are 7.289, 16.74, 25.57, 45.3, 56.0 eV. Atomic radius is 0.182 nm, radius of Bi3+ ion is 0.120 nm, of Bi3− ion is 0.213 nm. Electronegativity is ≈1.95. In the free form Bi is a silvery metal with a pink tint. Crystalline lattice is rhombohedral with the following parameters: a = 0.47457 nm and α = 57◦ 14 13 . Its density is 9.80 g/cm3 (at 293 K); density of the liquid form is 10.27 g/cm3 (at 544.4 K); T melting = 544.4 K, T boiling = 1833 K. Speciﬁc heat is 0.129 (at 293 K), in liquid state 0.142 (at 544.4 K), 0.148 (at 673 K), 0.166 kJ·kg−1 ·K−1 (at 1073 K); thermal coefﬁcient of linear expansion is 13.3·10−6 K−1 , volume expansion of metal upon solidifying +3.32% (at 544.4 K); thermal conductivity coefﬁcient is 8.374 W·m−1 ·K−1 (at 293 K), 15.491 (at 673 K); heat of melting is 11.38 kJ/mole; heat of evaporation 179 kJ/mole. Speciﬁc electrical resistance is 1068 μ·m (at 293 K), 1.602 (at 373 K), 1.289 (at 573 K), 1.535 (at 1053 K). The transition temperature T c of a superconducting thin ﬁlm state is ≈7 K. Under the inﬂuence of a magnetic ﬁeld the electrical resistance of Bi increases more than that of other metals so it is used for the measurement of strong magnetic ﬁelds. The tensile strength is 4.9 to 19.6 MPa, elastic modulus is 31.37 GPa, rigidity 12.35 GPa, Brinell hardness is 94.2 MPa, Mohs hardness is 2.5. Adiabatic elastic moduli of Bi in the hexagonal system, 3m (D3d ) class (room temperature): c11 = 63.7, c12 = 24.88, c13 = 24.7, c14 = 7.17, c33 = 38.2, c44 = 11.23 GPa. In the temperature range 423 to 523 K, bismuth compresses in a comparably easy manner. Bismuth is a diamagnetic metal with magnetic susceptibility −1.35·10−9 (upon melting the susceptibility

BLISTERING

decreases 12.5 times). Cross-section for thermal neutron capture is not high in Bi (0.034 barn). Bismuth is used for the production of low-melting alloys (e.g., Wood’s metal alloy with melting point of 343 K). Bismuth alloys are used in the helices of devices for measuring strong magnetic ﬁelds, and it also serves as a heat-transfer agent in nuclear reactors. BISTABILITY

A property whereby a system has two stable states in a certain region of variation of its parameters. The existence of bistability is connected with nonlinear properties of the system, and produces hysteresis during a fast enough variation of the parameters. It is exempliﬁed by optical bistability, polarization optical bistability, an N- or S-shaped current–voltage characteristic, the magnetic polarization of a ferromagnet, in a magnetic ﬁeld, etc. Nonlinear systems may exhibit more than two stable states (multistability). BITTER PATTERN See Magnetic powder pattern. BLACK-AND-WHITE GROUPS The same as Shubnikov groups. BLAHA–LANGENECKER EFFECT (F. Blaha, B.-Z. Langenecker, 1935)

Reduction of the force needed for plastic deformation of a specimen under simultaneous action of static and alternating loads.

117

The effect is observed in technological processes involving the shape-changing of metals (such as drawing, punching, rolling, and so on). The effect is especially noticeable when using ultrasound (see Ultrasonic treatment); in this case, the reduction of static stress depends on the ultrasound intensity, the nature and the condition of the material, the temperature, and other conditions. The effect of the ultrasound is explained by a local absorption of the energy of the high-frequency oscillation by various defects of the crystalline structure (see Defects in crystals), which facilitates the multiplication of dislocations and vacancies, as well as their motion in the crystal. BLISTERING

An appearance of blisters on a crystal surface under bombardment with atoms (ions) of inert gases, protons, and other particles. The blisters “ripen” with an increase in dosage (see Dosimetry) up to a stage when the blister dome breaks due to the increased pressure inside it. A new generation of blisters can develop on the uncovered area. The subsequent stages of the blistering are shown in the ﬁgure. The phenomenon of blistering is caused by migration of irradiationinduced vacancies and vacancy pores towards the surface. The mechanical stresses arising at embedding of the bombarding ions into the subsurface layer can also induce blistering. If the defect density is sufﬁciently uniform along the surface, the scabbing of thin plates off the surface of the irradiated material takes place instead of blister formation. The blistering and ﬂaking phenomena lead

Blistering process.

118

BLOCH EQUATIONS

to strong surface erosion of irradiated material at high irradiation doses. BLOCH EQUATIONS (F. Bloch, 1946)

Phenomenological equations describing the magnetic properties of ensembles of electrons (γ < 0) and nonzero-spin nuclei (γ > 0) in external magnetic ﬁelds:

χ = (ω0 − ω)T2 χ ,

Mx i + My j dM = γ (M × B) − dt T2 Mz − M0 − k, T1

χ = (1)

where Mx , My , Mz are the components of magnetization vector M; M0 is the equilibrium value of Mz ; i, j and k are the unit vectors of the laboratory coordinate system; B = kB0 + i2B1 cos ωt , B0 is the constant magnetic ﬁeld component directed along z axis; ω is the frequency; and B1 is the amplitude of alternating magnetic ﬁeld (B0 B1 ); γ is the gyromagnetic ratio. The constant T1 is called the longitudinal or spin–lattice relaxation time and T2 is the dephasing time, also referred to as the transverse or spin–spin relaxation time. In the general case, T1 is unequal to T2 (T1 T2 ) since T1 characterizes the rate of establishing thermal equilibrium between the spins and the lattice, while T2 is related to rate of establishing thermal equilibrium within the spin system, and this latter is equivalent to the decay rate of the phase coherences between precessing spins (as a result of the interaction between each other and with their environment, the spins precess in different local ﬁelds). The Bloch equations are based on the following reasoning. In an arbitrary uniform magnetic ﬁeld B the equation of motion of the magnetization vector M of the ensemble of free spins has the form dM/dt = γ (M × B). It is postulated that: (i) in a constant magnetic ﬁeld Bz , the longitudinal magnetization Mz relaxes to M0 in an exponential manner, i.e. satisﬁes the equation dMz /dt = −(Mz − M0 )/T1 ; (ii) transverse components Mx and My decay exponentially to zero as dMx Mx , =− dt T2

dMy My ; =− dt T2

(iii) in an external magnetic ﬁeld (comprised of a strong constant and weak alternating components) the relaxation motion of the magnetization vector is superimposed on the motion of free spins. Under the conditions of resonance, the stationary solutions of Eqs. (1) lead to the following expressions for the real (χ ) and imaginary (χ ) parts of the magnetic susceptibility:

(2)

−1 1 , γ M0 T2 1 + (ω − ω0 )2 T22 + S 2

where ω0 = γ B0 , χ determines the Lorentzian shape of the line with a half-width at a half-height of Δ = (1 + S)1/2 /T2 ; and the saturation factor (see Saturation effects) S = γ 2 B12 T1 T2 indicates the dependence of the line shape on the alternating ﬁeld intensity. In the absence of saturation (S 1), the half-width is determined by the spin– spin relaxation time T2 . The Bloch equations are also used for the analysis of pulsed experiments. One can obtain Eqs. (1) from the general theory of relaxation (see Bloch–Red eld theory). For twolevel systems they are valid if alternating ﬁelds are small and there are no spin–spin interactions. In solids the value of T2 is often estimated from the width. In this case Eqs. (1) lead to a discrepancy with the experimental data in the limit of strong saturation. Despite the limits to their applicability, the Bloch equations play an important role in elucidating many aspects of nuclear magnetic resonance and electron paramagnetic resonance in solids. BLOCH FUNCTION See Bloch theorem. BLOCH–GRÜNEISEN FORMULA (F. Bloch, E. Grüneisen, 1930)

An interpolating expression describing the temperature dependence of that part of electric resistance of metals ρT that is caused by electron scattering by lattice vibrations (phonons): 5 Θ/T z5 dz T ρT = 4 ρ0 , z Θ (e − 1)(1 − e−z ) 0

(1)

BLOCH LINE

where Θ is the Debye temperature, and ρ0 is a constant independent of temperature. In the simplest case of a spherical Fermi surface, the value of ρ0 is ρ0 =

ε2 3π m2 , 2 2 e n M0 v0 kΘ

(2)

where m is the electron effective mass, M0 is the atomic mass of a metal atom, v0 is the volume per atom, n is the density of conduction electrons, ε is a particular energy parameter (in the simplest case, the strain potential) characterizing the electron–phonon interaction; ε ∼ 1–10 eV. At high temperatures (T Θ), Eq. (1) has the form ρT = (T /Θ)ρ0 , i.e. it describes an ordinary linear growth of the metallic resistance with increasing temperature. At low temperatures (T Θ), Eq. (1) yields the wellknown Bloch law ρT ∼ T 5 , where ρT = 497.6(T /Θ)5 ρ0 . For a majority of simple metals the parameter Θ evaluated from Eq. (1) is in good agreement with the Debye temperature obtained from measurements of the speciﬁc heat. BLOCH LAW, three halves power law (F. Bloch, 1930)

The temperature T dependence of spontaneous magnetization Ms of ferromagnets in the temperature range signiﬁcantly lower than Curie point Θ, but higher than the magnon activation energy:

119

BLOCH LINE

A linear inhomogeneity of a 180◦ magnetic domain wall (Bloch wall) that separates wall re-

gions with different directions of magnetization rotation (see Fig.). The z axis is the Bloch line. A Bloch line cannot end anywhere in the domain wall, it either forms a closed ring, or terminates at the surface of the magnetic substance, i.e. the medium. The domain wall thickness decreases near the Bloch line, as shown. Bloch lines are distinguished according to their orientation. Vertical Bloch lines are directed normally to the surface of the magnetized material, and exist in domain walls of materials with magnetic bubble domains. They can be detected with the help of direct methods, such as electron microscopy or, in some cases by magneto-optic methods (see Magnetic domain characterization), and by the deformation of a moving domain wall at the location of an accumulation of vertical Bloch lines. Magnetic bubble domains with a large number of vertical Bloch lines (see Rigid magnetic bubble domain, Dumbbell domain) possess anomalous dynamic properties. S. Konishi (1983) proposed to use these lines for solid-state systems capable of superdense magnetic information recording. Horizontal Bloch lines that are directed parallel to the sample surface, as well as Bloch lines of a more involved shape, can arise during the motion of a twisted domain wall (see Domain wall twisting). Horizontal Bloch lines

T 3/2 , Ms = Ms0 1 − α Θ

where M s0 is the maximum value of M s at T = 0 K, and α is a constant which is speciﬁc for a given substance. This formula represents the ﬁrst terms of the expansion of M s (T ) in powers of T /Θ. The subsequent terms of the series are negligible (at T < Θ) and, as experiments show, the Bloch law is satisﬁed well up to T ≈ Θ/2. The decrease of M s with increasing T is a result of the disturbance of the ordered orientation of atomic (spin) magnetic moments in ferromagnets due to the thermal excitation of magnons. Their number grows as T 3/2 with increasing temperature, in accordance with the equation.

Distribution of magnetization indicated by solid arrows outside and within a domain wall with vertical (along z) Bloch lines; light arrows indicate directions of magnetization rotation.

120

BLOCH POINT

play an important role in the formation of the phenomenon of ballistic aftereffect in the motion of magnetic bubble domains. BLOCH POINT

A point inhomogeneity, a singular point of the magnetization M(r) at the merging of two Bloch lines of different signs in a magnetic domain wall.

The magnetization on a closed surface surrounding a Bloch point takes on all possible values. Thus, m = M/M s is equal to +ez and −ez far from the domain wall, to +ey and −ey in the middle of the domain wall far from the Bloch line, and to +ex and −ex in the middle of Bloch line segments of opposite sign (see Fig.). Hence, when approaching a Bloch point, the direction of magnetization m depends on the direction of approach, thus producing a “hedgehog”-type singularity of the magnetization ﬁeld (see Topological inhomogeneity). The following distribution corresponds to this singularity at a < r < Δ (a is the interatomic distance, Δ is the domain wall thickness): r (1) m=± , r where the different signs determine the sign (i.e. topological charge) of a Bloch point. There are other possible distributions that can be obtained

Distribution of magnetization indicated by arrows in a domain wall with a Bloch point BP crossed by Bloch lines BL-1 and BL-2.

from Eq. (1) by a uniform rotation. (The Bloch point in Fig. takes the form m = r/r after the rotation of m by π/2 about the y axis.) In materials with strong uniaxial magnetic anisotropy, the loss of domain wall energy due to the presence of a Bloch point is not signiﬁcant. Bloch points must always arise under certain distributions of the magnetization. Bloch points and their displacements under the action of an appropriately directed magnetic ﬁeld (along x axis) are detectable in domain walls of materials with magnetic bubble domains by the deviation of the direction of domain motion from the direction of the magnetic ﬁeld gradient (see Rigid magnetic bubble domain). BLOCH–REDFIELD THEORY

A magnetic resonance theory describing the time evolution of a spin system, located in an external magnetic ﬁeld, and interacting with its molecular environment (with the lattice). The main result of the theory is the Markovian kinetic equation for the spin density matrix. A consistent quantum-statistical derivation of the kinetic equation was ﬁrst presented by F. Bloch and R.K. Wangness, then Bloch generalized the theory for alternating magnetic ﬁelds of arbitrary magnitude. Later A.G. Redﬁeld put forth a semiclassical theory of relaxation where an approach to the calculation of the kinetic equation coefﬁcients was treated for the ﬁrst time. The basic physical concepts of the Bloch and Redﬁeld theories are the same. Later, both theories were described within the framework of a general formalism by other authors. Let a closed region comprise a spin system and a lattice with the Hamiltonian H = Hs + Hs (t) + Hsf +F where Hs is the time-independent Hamiltonian of the spin system, Hs (t) is the interaction operator of the spin system with alternating mag netic ﬁelds, Hsf = α uα vα is the spin–lattice interaction operator, uα are the lattice operators, vα are the spin operators, F is the Hamiltonian of the lattice. The exact equation of motion for the density matrix ρ of the closed system, idρ/dt = [H, ρ], is iterated in the interaction representation, and the inﬁnite series obtained is truncated at the second term (spin–lattice interaction considered as small perturbation). Then the spin density matrix evolves with the expression: σ = Trq ρ where the

BLOCH WALL

trace (Tr) of the matrix is taken over the lattice states. The kinetic equation for elements σmn has the following form: dσmn dt = i[σ, Hs + Hs (t)]mn + (2Γmkln σkl − Γklmk σln − Γlnkl σmk ). kl

(1)

Here the indices m, n, k, l enumerate the energy levels of Hamiltonian Hs ; jαβ (ωmk )vβmk vαln Δ(ωmk +ωln ), Γmkln = π

121

the density matrix σ changes insigniﬁcantly within the time tl , thus allowing one to apply perturbation theory); (iv) alternating magnetic ﬁelds are small; γ B1 τc−1 , γ B0 , where B1 is the amplitude of the external alternating magnetic ﬁeld, B0 is the amplitude of the externally applied magnetic ﬁeld, and γ is the gyromagnetic ratio; (v) the interaction between the lattice and the spin system results in a small shift of the levels of the latter that is ignored in Eq. (1); and (vi) the relaxation coefﬁcients Γ are time-independent and comparable to the reciprocals of the relaxation times.

αβ

where jαβ (ωmk ) is the Fourier transform of the lattice correlator: jαβ (ωmk )

=

−βFr δ(ω mk + ωrr ) r,r uαr r uβrr e , −βF 2πTrq e

where ωr r are the lattice eigenfrequencies; ωmk are the eigenfrequencies of the spin system; vβmk and vαln are the matrix elements with respect to eigenfunctions of Hamiltonian Hs ; uαr r and uβr r are the matrix elements of eigenfunctions of operator F ; β = /(k B T ), where T is the lattice temperature, Fr is the energy of rth lattice level. One must retain on the righthand side of Eq. (1) those Γmkln for which |ωmk + ωln | τc−1 . This is formally achieved by the introduction of the Heaviside step function Δ(x) = 1 at |x| < τc−1 and Δ(x) = 0 otherwise, where τ c is the lattice correlation time (perturbations in the lattice disappear within time τ c ). The derivation of the equation requires a number of assumptions: (i) the lattice stays close to thermal equilibrium; (ii) the inﬂuence of the spin system on the lattice is negligible, since the lattice has many more degrees of freedom than the spin system (ρ = σρf , where ρf is the equilibrium density matrix of the lattice); (iii) there exists a time interval t such that

t τ c and simultaneously t τ r , where τ r is the shortest relaxation time of the spin system (if the latter condition is met then

It follows from the relation Γmkln = Γlnmk exp(βωln ) ≈ Γlnmk exp(βωkm ) that in the absence of alternating magnetic ﬁelds, the solutions of Eq. (1) are elements of the equilibrium spin density matrix, i.e. due to the relaxation the spin system equilibrates with the lattice. Eq. (1) describes the magnetic resonance and the relaxation of magnetically dilute spin systems. BLOCH THEOREM

One of the most important theorems in solid state physics, which states that the intrinsic states of a particle in a periodic potential V (r) satisfying condition V (r + t) = V (r) (where t is the constant distance vector called the directlattice vector) can be characterized by two quantum numbers, viz., the band number λ and a realvalued vector k called the quasi-wave vector (lattice wave vector or crystal momentum). The wave function Ψkλ (r) called the Bloch function satisﬁes the condition Ψkλ (r + t) = Ψkλ (r) exp(ikt); and can be written as Ψkλ (r) = ukλ (r) exp(ikt) where ukλ has the symmetry of the potential, so that ukλ (r + t) = ukλ (r). The function Ψkλ (r) can also be written as a linear combination of Wannier functions Φλ (r), i.e. Ψkλ (r) =

ikr R e Φλ (r − R), where the set of points R transforms to itself upon displacement by the vector t , i.e. it possesses the symmetry of the potential. BLOCH WALL See Magnetic domain wall.

122

BLOCH WAVE FUNCTION

BLOCH WAVE FUNCTION See Bloch theorem. BLOCK STRUCTURE Partitioning a crystal into regions (blocks)

slightly disoriented relative to each another (disorientation angles are on the order of a few minutes of arc). Other terminologies are mosaic structure and blocks of mosaics (see Mosaic crystals). A block structure comprises disordered regions separated by closed small-angle boundaries in the form of dislocation interlacements, skeins, tangles, nets and dislocation walls of various structural and dislocation compositions. The regions contain both a cellular structure and a variety of dislocation structures such as individual dislocations, dislocation dipoles, multipoles, clusters, interlacements, wisps, nets, walls, and so on. The boundaries may be thin or thick, dense or rareﬁed, etc. The nets, boundaries, and walls may be regular or irregular; the networks may be hexagonal, tetragonal, etc. Incomplete (i.e. either forming or decaying) boundaries are a common occurrence. Depending on the dislocation composition and structure, the boundaries may be twisting or inclination ones, or a mixture of different varieties. The blocks may be equiaxial or nonequiaxial textured (see Texture). Block structures with smallangle boundaries composed of fairly regular nets and walls are often called polygonized structures. If the block size is commensurable with the grain size in a polycrystal, or with a single crystal size, the blocks are often called subgrains. The block size can vary from 0.1 to 10 μm. BLUE BRITTLENESS Lowering of the plasticity of unhardened construction steel at temperatures of blue color ir-

ridescence (300–500 ◦ C). It is responsible for the hardening of ferrite at temperatures about 300 ◦ C under conditions of static loading, and the formation of aggregations of impurity atoms which enhance its brittleness at temperatures about 400– 500 ◦ C under conditions of dynamic loading. In this case the plasticity is reduced owing to the formation of Cottrell atmospheres around dislocations because of the sharp growth of the diffusion rate as the temperature rises. In addition, under

conditions of shock loading, the velocity of dislocation motion exceeds that of impurity atom atmospheres. The latter start to lag behind the dislocations, forming elongated aggregations of impurity atoms, which extend in the direction of the steel plastic ﬂow. The presence of such aggregations in steel ferrite increases the alloy brittleness. Blue brittleness is reduced in steel by introducing elements linking interstitial atoms in carbides and nitrides. BLUE PHASES of liquid crystals Phases existing in a narrow temperature range

(1–0.1 ◦ C in order of magnitude) between a liquid phase and a cholesteric phase (see Cholesteric liquid crystal), possessing a spatial three-dimensional periodicity, and formed by bilaterally asymmetric elongated molecules. Three blue phases are known, designated as BPI, BPII, and BPIII, with no translational long-range order present in the highest-temperature phase BPIII of the group (see Long-range and short-range order). In view of the bilateral symmetry of phases BPI and BPII, a coil twisting is locally advantageous in two directions (in spite of the single direction where it takes place in a cholesteric). Therefore, a three-dimensional lattice of linear defects (disclinations) with a period 0.5 μm appears in the system. Thus, blue phases are the analogues of ordinary solid crystals where the structural elements are not the individual atoms or molecules, but the cells of the disclination network. There also exist some other models of blue phases. The positions of the molecules themselves are not ﬁxed; only their orientations are conserved at every point. Despite the lack of any direct proof of the existence of the disclination lattice in a blue phase, there are some indirect effects arguing in favor of the model, such as the increase of the lattice period with a decrease in the temperature. Due to a periodic structure, the BPI and BPII are able to form well-faceted monocrystals, and also to selectively scatter light in a visual spectral range, thus acquiring the blue color that gives them their name. Two optical characteristics of the BPI and BPII phases are the strong rotation of the light polarization plane (arising due to a coil structure) and the lack of linear double refraction (due to the cubic form of the disclination network cells). Although blue phases

BOGOLYUBOV METHOD

have been well known since the discovery of liquid crystals in 1888, nowadays these phases are among the least studied liquid crystals. BODY-CENTERED LATTICE, I -lattice

A lattice whose unit cell parallelepiped contains an extra site in the cell center (see Bravais lattices) as well as the sites at the vertices. In addition to the three basic translations a, b, c, the lattice possesses a further translation t = (a + b + c)/2. The latter can appear only in rectangular parallelepipeds; therefore, body-centered lattices exist only in orthorhombic, tetragonal, and cubic crystallographic systems. In triclinic and trigonal crystal systems the I-lattice reduces to a smaller primitive lattice (see Primitive parallelepiped). In a monoclinic crystal system, this is a base-centered lattice with the unit cell volume and other basis translations half as large. In the hexagonal lattice case, the appearance of the translation t leads to a lowering of the symmetry to that of a monoclinic base-centered lattice. Considering the point symmetry of the sites, the body-centered lattice belongs to the body-centered Bravais groups. BOGOLYUBOV CANONICAL TRANSFORMATIONS

See Canonical transformation method. BOGOLYUBOV–DE GENNES EQUATIONS (N.N. Bogolyubov, 1958; P.G. de Gennes, 1963)

Equations of the mean eld approximation in the theory of superconductivity that determine the energy eigenvalues ελ and the correspond (r) of Boing two-component wave functions uv λ(r) λ golyubov quasi-particles (see Bogolyubov method) in a spatially inhomogeneous state of a superconductor described by the order parameter Δ(r) = g(s −s ). Here s (r) is the annihilation operator of an electron with spin s, and g is the matrix element of the effective electron–electron interaction in Bardeen–Cooper–Schrieffer theory. These equations have the form: 0 uλ (r) + Δ(r)vλ (r) = ελ uλ (r), H ∗ vλ (r) + Δ∗ (r)uλ (r) = ελ vλ (r), −H 0

123

where 0 = 1 −i∇ − eA(r) 2 + U (r) − E F H 2m is the one-electron Hamiltonian of the normal state of a metal, m is the electron mass, A(r) is the magnetic ﬁeld vector-potential, U (r) is the effective one-particle potential for the electrons in the metal, and E F is the Fermi energy. In the thermodynamic equilibrium state, the value of Δ(r) satisﬁes the self-consistency condition ελ . uλ (r)vλ∗ (r) tanh Δ(r) = g 2kB T λ

The Bogolyubov–de Gennes equations were used to solve spatially nonuniform problems of superconductivity theory such as, e.g., calculation of the upper critical eld B c2 (T ), ﬁnding the excitation spectrum in the vortex lattices, determining the boundary conditions in proximity effect theory, elucidating particular features of the reﬂection of quasi-particles from a “normal metal– superconductor” interface (see Andreev re ection of quasi-particles), ﬁnding the excitation spectrum in S–N–S contacts, etc. BOGOLYUBOV METHOD in the theory of superconductivity (N.N. Bogolyubov, 1958)

A ﬁeld theory method for calculating the ground state energy and the spectrum of single particle and collective excitations in superconductors. The initial Hamiltonian of the electron and phonon subsystems of a metal was diagonalized using the unitary transformations of creation and annihilation operators of bosons and fermions (see Canonical transformation method) and the principle of renormalization, i.e. the compensation of divergent Feynman diagrams by a perturbation theory series. The Bogolyubov method is an alternative to the variational method in Bardeen– Cooper–Schrieffer theory and, unlike the latter, allows a consistent treatment of collective effects and the Coulomb interaction in superconductors. In particular, within the framework of the Fröhlich Hamiltonian for the electron–phonon interaction, this method was used to obtain in the

124

BOGOLYUBOV–TOLMACHYOV LOGARITHM

weak coupling limit, for the ﬁrst time, an equation for the energy gap parameter Δ in the spectrum of a superconductor taking into account effects of retardation. In addition, with the help of the Bogolyubov method, a further weakening of the screened electron–electron repulsion was shown to exist (see Bogolyubov–Tolmachyov logarithm), which facilitates Cooper pairing due to the electron–phonon interaction. When the Bogolyubov method was applied to collective excitations involving undamped branches in the energy range √ ω < 2Δ with a linear dispersion law ωq = qv F / 3 (where v F is the Fermi velocity), they were found to exist in neutral superﬂuid Fermi systems. That branch represents a Goldstone mode. In charged Fermi systems with longrange Coulomb repulsion (electrons in a metal), the branch transforms into plasma oscillations with the frequency ωq = 0 at q → 0. BOGOLYUBOV–TOLMACHYOV LOGARITHM (N.N. Bogolyubov, V.V. Tolmachyov, 1958) The logarithm of the ratio of the Fermi energy in metals E F ∼ 1–10 eV to the mean energy of phonons ωD ∼ 0.1–0.01 eV (ωD is the Debye frequency) that characterizes the extent of the ef-

fective weakening of the Coulomb repulsion between the electrons in a superconductor: c = V

Vc , 1 + N(0)Vc ln[EF /(ωD )]

where V c is the matrix element of the screened Coulomb interaction that is averaged over the Fermi surface, and N(0) is the density of states at the Fermi level. The extra (relative to screening) weakening of the repulsion is caused by the decreased probability of the appearance of two electrons within the limits of the screening region due to Coulomb scattering. It facilitates electron Cooper pair formation via an effective attraction, which results from virtual phonon exchange. BOHR MAGNETON See Magneton. BOHR RADIUS

The radius a B of the orbit of an electron in the ground state of a hydrogen atom.

More generally, the distance between the center of the hydrogen atom and the maximum of the quantum-mechanical probability for detecting an electron; or the distance through which the electron wave function reduces by the numerical factor of e = 2.71828. The Bohr radius has the value a B = 4πε0 2 /(me2 ) = 5.2918·10−11 m, where m and e are the electron mass and charge, respectively, = h/(2π) is the reduced Planck constant. In the physics of insulators and semiconduc∗ is used which tors the effective Bohr radius aB differs from the Bohr radius a B with m replaced with the effective mass of an electron in a crystal √ and e replaced by the effective charge e∗ = e/ ε, where ε is the relative dielectric constant. The effective Bohr radius determines the approximate ∗ n2 ) dimensions and energy, En = −e∗2 /(8πε0 aB (where n is the principal quantum number), of shallow hydrogen-like centers and Wannier–Mott excitons in semiconductors. It is a convenient scale for expressing the dimensions of localized electron states in nonmetallic crystals. BOHR–VAN LEEUWEN THEOREM (N. Bohr, 1911; generalized by J. van Leeuwen, 1919)

A theorem of classical statistical physics, which states that the magnetization of a system of charged particles in a constant external magnetic ﬁeld under the conditions of statistical equilibrium is equal to zero. The theorem demonstrates that it is impossible, within the framework of the classical statistical mechanics of charged particles, to explain ferromagnetism, paramagnetism and diamagnetism. As was shown later, the magnetism of a substance is caused by quantum properties of the particles comprising it. BOLOMETER

A device for measuring the radiated energy (power) in the infrared and optical wavelength ranges. It is in common use for various detection schemes with narrow ranges of extreme sensitivity to particular excitations. It was ﬁrst used by S. Langley (1880) for measurements in the IR range of the solar spectrum. The principle of bolometer operation is based on the change of the resistance of the thermosensitive element under the action of radiation. Bolometers are nonselective optical radiation detectors. To

BOLTZMANN EQUATION

obtain equivalent spectral sensitivity in a given range, absorbing coatings are applied to the sensitive elements of the bolometer. There are metallic, semiconductor (thermistor) and insulator bolometers. The use of cryogenic effects allowed producing cooled bolometers based on the conduction of shallow levels in semiconductors, as well as superconducting (isothermal and nonisothermal) bolometers. BOLTZMANN CONSTANT (L. Boltzmann)

One of the fundamental physical constants, a parameter of the statistical Boltzmann distribution and Gibbs distribution. Through them, the Boltzmann constant k B enters various thermodynamic relations, for example, it relates the thermodynamic probability W of a system state to the entropy S through the expression S = k B ln W , and determines the mean thermal energy k B T /2 of a particle per degree of freedom. The gas constant R involved in the equation of state for one mole of the ideal gas, pV = RT (p is pressure, V is gas volume), is related to the Boltzmann constant by k B = R/N A , where N A is the Avogadro number. The standard value based on the 1986 CODATA recommendations is k B = 1.38066·10−23 J/K. BOLTZMANN DISTRIBUTION A distribution function of coordinates and momenta for particles or quasi-particles of an ideal

nondegenerate gas in the state of thermodynamic equilibrium. The probability dW of a particle to have a momentum in a range p ⇒ p + dp and a coordinate in a range r ⇒ r + dr is related to the Boltzmann distribution fn (r, p) by dW (r, p) = fn (r, p) dr dp, where in the classical case we have the approximation ε(p) + U (r) . (1) fn (r, p) = A exp − kB T Here ε(p) is the kinetic energy, U (r) is the potential energy, k B is the Boltzmann constant, and A is the normalization factor found from the condition that the probability of a particle to be present in the phase space equals unity, i.e. W = dW = 1. Sometimes the following expression obtained by

125

integrating Eq. (1) over all momenta p is referred to as the Boltzmann distribution function: U (r) f (r) = A exp − , kB T while Eq. (1) is called the Maxwell–Boltzmann distribution. Integration of Eq. (1) over coordinates yields the Maxwell distribution of velocities. In a quantum description of particles characterized by a set of single-particle energy levels Ei , the Boltzmann distribution takes the form μ − Ei , (2) ni = exp kB T where ni is the average number of particles in the state with energy Ei , μ is the chemical potential of the system that acts as the normalization factor

determined by setting the sum i ni equal to the total number of particles, N . The Boltzmann distribution is the high temperature limiting case of the more accurate Bose–Einstein and Fermi–Dirac distribution functions (see Bose–Einstein statistics, Fermi–Dirac statistics) that take into account the quantum character of particle motion, and this limiting case is valid for an ideal gas with a small density of particles at high temperatures. In the physics of semiconductors, the Boltzmann distribution is widely used in the statistics of a gas of quasi-particles (electrons and holes) to determine their equilibrium concentrations and other speciﬁc parameters. BOLTZMANN EQUATION (L. Boltzmann, 1872) An integro-differential kinetic equation that

provides the time (t) evolution of the one-particle distribution function (f ) of a low-density monatomic gas. The Boltzmann equation has the form ∂f 1 + (p, ∇x f ) + (F, ∇p f ) = ρLp (f, f ), ∂t m where f (x, p, t) is the probability density function in the phase space of coordinates and momenta of a particle (x, p), m is the particle mass, F is the external force ﬁeld applied at the point (x, p) of the phase space, and ρ is a dimensionless parameter proportional to the mean density of gas particles. The collision operator (or collision

126

BOND

integral) Lp has the following form: 1 Lp (f, f ) = dp dσ |p − p | m × f (p∗ )f (p ∗ ) − f (p)f (p ) , where the explicit dependence of the function f on the coordinates and time is omitted, and dσ is the differential cross-section which includes conservation laws of both energy and momentum. Momenta p∗ , p ∗ can be found from solving the scattering problem for two particles with incident momenta p and p and a certain impact parameter, colliding in accordance with the laws of classical mechanics. When deriving the Boltzmann equation, the evolution of the function f (x, p, t) within a small time interval is assumed to be determined by its value at a given instant of time t by means of the free motion of gas molecules and their pairwise collisions, provided the interaction time during the collision of two gas particles is much smaller than their mean free path time. The operator Lp is constructed taking into account the number of particles in a phase volume element. The Boltzmann equation is derived from the Liouville equation in the lowest-order approximation using an expansion in powers of the density. If a system is in statistical equilibrium the collision integral vanishes, and the Maxwell distribution will be a solution to the Boltzmann equation. BOND

See Chemical bonds, Covalent bond, Hydrogen bond, Ionic bond, Ionic-covalent bond, Metallic bond. BOOJUM A point defect in the ﬁeld of a director at the boundary of a nematic (see Nematic liquid crystal).

Boojum-induced elastic distortion spreads over the entire bulk medium. Displacement of a boojum into the bulk is energetically unfavorable because a boojum in this case would be a point defect connected to the surface, i.e. a disclination. The director distribution in the vicinity of a boojum depends on the orientation of nematic molecules near the boundary. When this orientation changes, e.g., as shown in the ﬁgure, from a tangential orientation to a normal one, a boojum can either disappear or transform into a hedgehog and move from the sur-

Change in the director distribution during the transformation of a boojum into a hedgehog (above), and into a uniform state (below), during the variation of the director angle relative to the surface. Each distribution is axially symmetric, and the ﬁgure presents sections in a vertical plane.

face to the interior. Experimentally, boojums are observable in plane textures of liquid crystals in the form of defect points at the sample surface as well as in spherical nematic drops. The boojum was ﬁrst studied by N.D. Mermin (1976) in superﬂuid 3 He-A. The nature of the ordering in the latter is similar to that in nematic liquids (see Super uid phases of 3 He). BORN APPROXIMATION (M. Born, 1926)

A quantum mechanical perturbation theory method of calculating the probability of scattering of a particle (quasi-particle) off a distancedecaying potential V (r). It is based on using plane waves for both the initial wave function prior to scattering, and the ﬁnal wavefunction far beyond the range of V (r) after scattering. The scattering amplitude in ﬁrst order perturbation theory (ﬁrst Born approximation) is m e−i(k−k )r V (r) d3 x, Akk = − 2 2π where m is the scattered particle mass, and k and k are the wave vectors of the incoming and scattered states of the particle, respectively. Subsequent orders of perturbation theory take into account the deviation of the wave function of the particle from a plane wave, which is caused by the interaction potential. The criterion of the Born approximation is |V (R)| 2 /(mR 2 ), where R is the range of the interaction potential. For an electron scattering off a Coulomb potential, the criterion of the Born approximation is v v (v is the relative velocity of colliding particles, v is the velocity of electron motion in the Bohr

BORON

orbit (see Bohr radius), v = Ze2 /(4πε0 ) (Z is the atomic number, e is the electron charge). The Born approximation ﬁnds wide use in the theory of current-carrier scattering and scattering of other microscopic particles in solids, in the treatment of ionization processes, e.g., light absorption by local electron centers (see Local electronic levels) in nonmetallic crystals, etc. BORN–HABER CYCLE (M. Born, F. Haber, 1919)

A method of approximate determination of the atomic bond energy in crystals (mainly alkalihalide crystals) from experimental data on reaction energies whose sequence (cycle) results in the formation of a crystal from its gaseous atoms. The bonding energy at the temperature of absolute zero is determined as a sum of energies needed for (i) heating the crystal to room temperature (1.5 to 3 kcal/mole); (ii) separating the crystal into the pure metal and the diatomic halide gas (60 to 150 kcal/mole); (iii) sublimation of the metal (20 to 40 kcal/mole); (iv) dissociation of the halogen into a monatomic gas (25 to 30 kcal/mole); (v) cooling the gases to absolute zero (to 2.9 kcal/mole); (vi) removing the valence electrons from alkali atoms (90 to 120 kcal/mole); (vii) formation of negative halide ions from atoms and electrons (70 to 80 kcal/mole). As a result of summing, the bonding energy turns out to equal ∼180 kcal/mole for LiI, ∼185 kcal/mole for NaCl, ∼170 kcal/mole for KCl, ∼160 kcal/mole for KBr, ∼145 kcal/mole for CsI, and so on. Application of methods similar to the Born–Haber cycle allows one to estimate the energies of various reactions in solids, which can be included into one or another cycle, using the known energies of other components of the cycle, e.g., from the energy of formation of Frenkel pairs (see Unstable Frenkel pair) or Schottky pairs in different charge states (see Schottky defect). BORN–VON KÁRMÁN BOUNDARY CONDITIONS (M. Born, Th. von Kármán, 1912)

Periodic boundary conditions imposed on the Bloch function of a particle in a periodic potential, or on a plane wave ϕ(x + Lx , y, z) = ϕ(x, y + Ly , z) = ϕ(x, y, z + Lz ) = ϕ(x, y, z),

127

where Li = Ni ai , i = x, y, z, are the Cartesian coordinates; ai and Ni are the crystal lattice constant and the number of lattice periods in the direction i, respectively. Born–von Kármán boundary conditions allow one to determine the number of allowed states of electrons with different quasiwave vectors k in a unit volume of the reciprocal space. Then, an extra (in addition to the Bloch theorem) condition ψkλ (r + L) = ψkλ (r) (where L is a linear combination of vectors L1 , L2 , and L3 with integer coefﬁcients) is imposed on the wave function. Hence, the number of allowed k values equals the number of unit cells in the volume V = L1 × L2 × L3 and the density of permitted states in k -space equals V /(2π)3 . None of the observed values, including the density of electron states referred to one unit cell, or per unit volume of direct space, are dependent on the selection of L1 , L2 , L3 or V . BORON, B

A chemical element of Group III of the periodic system with atomic number 5 and atomic mass 10.81. The isotope composition of natural boron: 10 B (19.57%) and 11 B (80.43%); the radioactive isotopes 8 B, 12 B and 13 B are known (halflives are fractions of a second). Outer electronic shell conﬁguration is 2s 2 2p1 . Successive ionization energies are 8.298; 25.16 and 37.93 eV. Atomic radius is 0.091 nm; ionic radius of B2+ is 0.023 nm. The most typical oxidation state is +3, and in compounds with metals −3 (borides). In the free state boron exists in the form of brown ﬁne-crystal powder (so-called amorphous boron) and of dark-gray crystals (crystalline boron). The most important boron modiﬁcations are simple α-rhombohedral B (I), tetragonal B (II), and complicated β-rhombohedral B (III). The α-rhombohedral boron lattice parameters are: a = 0.506 nm, α = 58.1◦ , density is 2.365 g/cm3 ; the tetragonal boron lattice parameters are a = 1.012, c = 1.414 nm, and the density is 2.365 g/cm3 ; for β-rhombohedral boron we have: a = 1.014 nm, α = 65.3◦ , density is 2330 kg/m3 . The modiﬁcations B (I) and B (II) under heating above 1773 K irreversibly transform to B (III). T melting of B (III) is 2346 K; T boiling is around 3973 K; thermal coefﬁcient of the linear expansion is

128

BORON CARBIDE

(1.1–8.3)·10−6 K−1 (from 293 to 1023 K). Thermal conductivity coefﬁcient of crystalline boron is 25.96 W·m−1 ·K−1 (at room temperature); speciﬁc heat of amorphous boron is 12.97 J·mole−1 ·K−1 , speciﬁc heat of rhombohedral boron is 11.1 J·mole−1 ·K−1 . Standard enthalpy is 5.895 J·mole−1 ·K−1 for crystalline boron and 6.548 J·mole−1 ·K−1 for amorphous boron; Debye temperature is 1220 K. Crystalline boron is a semiconductor; the forbidden gap width determined from electrical and optical measurements is 1.42 and 1.53 eV, respectively. Boron is a diamagnet, with speciﬁc magnetic susceptibility −0.62·10−9 (at room temperature). It is characterized by high hardness. At low temperatures, boron is a brittle material; above 1800 ◦ C, it begins to deform plastically. Chemically, boron is a nonmetal. Elementary boron has low chemically activity: in the air it burns at 973 K, forming B2 O3 ; with nitrogen above 1473 K, it forms boron nitrides; with carbon above 1573 K, it forms boron carbides. It does not interact directly with hydrogen, but a whole number of hydride compounds Bn Hm is known (see Hydrides), obtained indirectly using silicon. Above 1273 K, there are silicon borides; formed with phosphorus and arsenic above 1173 K are phosphides and arsenides. It ﬁnds wide application in the production of materials (boroplastics), hightemperature strong and superhard materials (e.g., borazon), neutron-adsorbing materials for nuclear power engineering, semiconductor materials, corrosion resistant and antifriction coatings. BORON CARBIDE, B4 C

The only chemical compound of boron with carbon with a broad homogeneity range (molar content of C is 8.6 to 21%). It forms a rhombo5 ), and the hedral lattice of space group R3m (C3v parameters of the crystal lattice in the homogeneity range vary from a = 0.5602 to 0.5616 nm, c = 1.2066 to 1.2120 nm. T melting = 2400 ◦ C, density is 2.51 g/cm3 , thermal conductivity is 121.4 W·m−1 ·K−1 at 300 K, microhardness is 45.0 GPa, elastic modulus is 450 GPa. Boron carbide is a semiconductor of p-type, band gap width is 0.84 eV, electrical resistivity is 0.01 ·m. Boron carbide does not decompose in mineral acids and alkalis. It is obtained through interaction of B2 O3

with coal in arc furnaces, by synthesis from the elements, by crystallization from melts, from their gaseous compounds. Boron carbide is used as an abrasive material, for the borating of metals and alloys, for adsorption of neutrons. BORON NITRIDE, BN

Chemical compound of boron with nitrogen, with three modiﬁcations: α-BN, β-BN, γ -BN. The α-BN compound is hexagonal with space 4 ), crystal lattice paramegroup P 63 /mmc (D6h ters: a = 0.2504 nm, c = 0.6661 nm; β-BN is ¯ cubic with sphalerite-type space group F 43m 2 (Td ), a = 0.3615 nm; γ -BN has the hexagonal wurtzite-like structure, space group P 63 mc 4 ), a = 0.255 nm, c = 0.423 nm. The α-BN (C3v compound transforms into β-BN under high pressure and temperature (P [kbar] = 11.5 + 0.025T ). In the course of heating under normal conditions, β-BN transforms to α-BN at temperatures above 1400 ◦ C; α-BN transforms to γ -BN at shock compression 120 to 130 kbar. The density is 2.20 g/cm3 for α-BN, 3.45 g/cm3 for β-BN and 1.8 g/cm3 for γ -BN; the thermal conductivity is 21 W·m−1 ·K−1 for α-BN and 1800 W·m−1 ·K−1 for β-BN. Microhardness of β-BN is 60 GPa; elastic modulus is 953 GPa. Boron nitride is an insulating material with electrical resistivity ρ > 1015 ·m and band gap width of β-BN ∼10 eV. Boron nitride is obtained by nitration of boron. The α-BN form is used as ﬁreproof and electrical insulating materials; β-BN is a tool and abrasive material. Cubic boron nitride is a superhard material having no natural analogs. It was obtained by Robert H. Wentorf, Gr. (1956) under high pressure (above 4.0 GPa) and temperature (above 1470 K) from hexagonal boron nitride in the presence of alkali and alkali-earth metals, lead, antimony, tin and nitrides of the said metals. The rules of formation of binary compounds with a tetrahedral conﬁguration are as follows. The components should belong to groups equidistant from Group IV of the periodic system; the average number of valence electrons in this compound should equal four. The majority of binary alloys with sphalerite and wurtzite structures satisfy these rules. Cubic boron nitride with sphalerite-type (β-BN) and wurtzite-type (γ -BN) lattices are characterized by

BOSE–EINSTEIN CONDENSATION

the tetrahedral arrangement of atoms with each atom of one type surrounded by four atoms of the other type. In β-BN and γ -BN lattices the four B–N bonds have the same length 0.157 nm, with 109.5◦ angles between them. The crystal lattice of β-BN is similar to that of diamond with spacing 0.3615 nm. Cubic boron nitride is an insulator with a density ≈3.465 g/cm3 . Nanotubes can be made from boron nitride. BORRMAN EFFECT The same as Anomalous passage of X-rays. BORRMAN TRIANGLE (G. Borrman)

A triangle in the scattering plane with one apex lying in the entry surface of a crystal, the two side lines directed along the wave vectors of the incident wave K 0 and the Bragg-diffracted wave K d (see Bragg diffraction), respectively, and the base formed by the segment of the exit surface of the crystal intercepted by these lines. If an X-ray beam is incident along K 0 at a certain point on the entry surface, and the crystal is oriented for Bragg reﬂection, then the wave ﬁeld inside a thin crystal propagates only within the Borrman triangle. Inside a Borrman triangle the response functions also have ﬁnite values (see Dynamic radiation scattering). BOSE CONDENSATE

A macroscopically large number of particles with integer spin (bosons) in an ideal or slightly nonideal Bose gas, which are in their lowest state with zero point energy and momentum at a temperature below the Bose–Einstein condensation temperature. Since the Pauli exclusion principle does not apply, bosons can accumulate in the lowest energy quantum state, all with the same energy forming a coherent condensate. The latter is described by a common complex wave function Ψ = |Ψ |eiΘ with a magnitude |Ψ | and phase Θ that are constant or slowly varying in time. This fundamental property of bosons underlies the phenomena of super uidity in liquid 4 He (see Bose u id) and superconductivity in metals (see Cooper pairs). Related to this is the possibility of laser generation (see Lasers) of a macroscopically large number of photons with the same wavelength under the conditions of a nonequilibrium inverted

129

level population, as well as the possibility of such

an accumulation of photons in a resonator. An analog of a Bose condensate is the ground state in systems with spontaneous symmetry breaking, which is described by a complex order parameter, in particular, the so-called Higgs ﬁeld (see Higgs mechanism). BOSE CONDENSATION The same as Bose–Einstein condensation. BOSE–EINSTEIN CONDENSATION, Bose condensation

The property of Bose particles (bosons) with integer spins to accumulate in macroscopically large amounts in a single quantum state described by a unique (coherent) wave function (see Bose condensate). Bose–Einstein condensation is a property of three-dimensional Bose systems only. It is missing in two- and one-dimensional systems. Bose–Einstein condensation of excitons and biexcitons is a variety this condensation for the case of quasi-particles (excitons and biexcitons, between which repulsion forces dominate). Bose– Einstein condensation of excitons interacting with phonons leads to renormalization of the energy spectrum of both subsystems and alters the shape of light absorption and luminescence bands. The bands contain additional sharp peaks generated by a condensed phase and sloping wings arising from condensate-free excitons. The Fermi nature of electrons and holes forming excitons leads to the non-Boseity of exciton operators. Excitons metallize when their concentration nex becomes −3 of comparable to the inverse of the volume aex the exciton, where aex is its Bohr radius. The Bose–Einstein condensation of excitons is realiz3 < 1 only. able under the condition naex Bose–Einstein condensation of dipole-active excitons and photons (or polaritons with wave vector k0 = 0) is of special interest. In this case, the Bose-condensed state can be considered as an intense coherent wave described by a coherent Glauber state with a macroscopic amplitude. Equations describing inhomogeneous in space and time weakly of excitons and of photons have been derived; the diagram techniques for nonequilibrium states has been developed to describe coherent quasi-particles existing simultaneously with

130

BOSE–EINSTEIN STATISTICS

a condensate. On this basis, the features of coherent nonlinear propagation of light in densely condensed media are assigned to the exciton spectral range. The values of wave vectors and frequencies have been found, where, due to the absolute and convective instability of the spectrum, generation and ampliﬁcation of waves is possible. Rearrangement of the energy spectrum of the phonoriton type (see Phonoriton) is due to peculiarities of the distribution functions of incoherent quasi-particles and conditions of stimulated Brillouin scattering of light. The role of quantum ﬂuctuations and the inﬂuence of incoherent polaritons upon the statistical properties of an intense polariton wave have been clariﬁed. A stimulated Bose– Einstein condensation of excitons and polaritons under the action of coherent resonant laser radiation, and a stimulated Bose–Einstein condensation of biexcitons obtained by two-photon excitation with counter-directed or parallel laser beams, were experimentally carried out. BOSE–EINSTEIN STATISTICS (Sh. Bose, A. Einstein, 1924)

The statistics describing the distribution in quantum states of a system of very many identical particles with zero or integer (in units) spin. Particles as well as quasi-particles that obey Bose–Einstein statistics are called bosons; including photons, phonons, magnons, excitons, bipolarons, π -mesons, and so on. The wave function of bosons is symmetric with respect to the exchange of any pair of particles. A particular feature of bosons is the possibility for any number of them to be in the same quantum state. In view of this property, it follows from the Gibbs distribution that the average number of particles ni in quantum state i with energy εi for a boson ideal gas (Bose gas) in thermodynamic equilibrium is −1 εi − μ −1 ni = exp , (1) kB T where k B is the Boltzmann constant, μ is the chemical potential determined by the total

number N of particles in the system, and N = i ni (μ). In a system with a variable number of particles, μ = 0; under constant N , μ < 0. Eq. (1) is called the Bose–Einstein distribution. At low temperatures, a ﬁnite portion of the particles pass to

the lowest states with ε = 0; their number N0 = N[1 − (T /T0 )3/2 ] where N 2/3 2 3.31 T0 ∼ = gV mk is called the condensation temperature, g is the degeneracy factor, m is the particle mass, V is the system volume. Other particles are distributed over states according to Eq. (1) at μ = 0. Such a transition is called a Bose–Einstein condensation (Bose condensation). The Bose–Einstein distribution determines the efﬁciency of scattering of particles moving in a solid (electrons and holes, neutrons, photons etc.) by photons, nonradiative quantum transitions in solids, phonon–phonon interactions and also values of electrical conductivity and thermal conductivity, speci c heat, acoustical properties, parameters of optical bands, spectral composition of black body radiation, and so on. BOSE FLUID A quantum liquid that condenses at low tem-

peratures and consists of interacting bosons, i.e. particles with integer (in units) intrinsic angular momentum (spin). An example of a Bose ﬂuid is liquid helium (4 He) at T < 4.2 K. Below some critical temperature (see Lambda point) Bose ﬂuids can transform into the superﬂuid state (see Super u idity). BOSE GAS (Sh. Bose)

A quantum system of weakly interacting particles (quasi-particles) with integer spins (bosons) subject to Bose–Einstein statistics with the distribution function (at spin σ = 0) −1 ε −μ −1 , nk = exp k kB T where εk is the energy of the kth quantum state or of a free particle with momentum k, μ is the chemical potential (μ 0), T is the absolute temperature. A Bose gas of neutral particles is ideal for a small density n, when n1/3 r0 1, where r0 denotes the action radius of exchange or van der Waals forces, and a Bose gas of electrically charged bosons (e.g., bipolarons) becomes weakly nonideal at a high density, when n1/3 a0 1, where a0 denotes the Bohr radius of particles. In

BOUNDARY EFFECTS

a Bose gas with a given (constant) number of particles, under a pronounced decrease of temperature, Bose–Einstein condensation takes place, while in a Bose gas with a variable number of particles (quasi-particles) determined by the thermodynamical (thermal) equilibrium condition (e.g., the phonon gas in a crystal or in liquid helium), the Bose–Einstein condensation does not occur. BOSE STATISTICS The same as Bose–Einstein statistics. BOTTLENECK OF PHONONS See Phonon bottleneck. BOUNDARY DIFFUSION Diffusion over two-dimensional structural defects like grain boundaries and subgrains, i.e. over

elements of imperfection of the crystal structure which separate parts of a bulk metal from crystal lattices of different space orientation, different crystal structure, or different material composition. Among the various types of boundary diffusion, the greatest interest involves material transfer over grain boundaries in polycrystalline materials. Boundary diffusion deviates from the usual Arrhenius linear dependence (see Interdiffusion) of log D versus 1/T where D is the diffusion coef cient; lower temperatures and grain pulverization result in greater departures from the Arrhenius law. The boundary diffusion coefﬁcient in metals is usually several orders of magnitude higher than that for bulk diffusion. A model for quantitatively estimating diffusion parameters put forward by I.C. Fisher (1951) provides the expression 0.21(D/t)1/2 , tan2 α where D GB is the diffusion coefﬁcient over the grain boundaries, t is the diffusion time, δ is the width of the boundary layer, and α is the slope of the straight line characterizing the dependence of the logarithm of the concentration on the diffusion depth. According to various authors the width of the boundary layer lies in the range from 0.3 nm to a few μm. The boundary layer has a so-called diffusion width, i.e. a region in which the mobility of atoms is higher than in the bulk. This width is approximately double the distance from DGB δ =

131

the grain boundary to the point where the diffusing atom concentration is reduced by the factor of e = 2.718 from its maximum value. For some metals (e.g., for self-diffusion in nickel) this distance is 4 to 5 μm. Diffusion over a phase boundary is of great importance for phase transition kinetics. On a phase boundary, like on a grain boundary, a change of the crystal lattice state, defect clustering, and chemical segregation are possible factors that enhance the atomic mobility compared to that in the bulk. The principal methods for investigating grain diffusion are macro-, micro- and electron microscopic autoradiography, and the method of secondary ion–ion emission. BOUNDARY EFFECTS in liquid crystals

Effects caused by the action of anisotropic surface forces. In technological applications and in laboratory studies liquid crystals are in contact with substrates and hosts (glass, polymers, isotropic liquids, cleavages of monocrystals, and so on). Anisotropic interphase interactions caused by the mutual action of various molecular forces (dispersion, dipole–dipole, steric) orient the molecules of a liquid crystal either normal to the boundary (homeotropic orientation), at an angle (conical or tilted orientation), or in the plane of the boundary (planar orientation). A quantitative measure of the orienting action of the substrate (i.e. of the external medium) on the liquid crystal is the cohesion energy (anchoring energy) W . The magnitude of W determines the work needed to turn the director (molecules) of the liquid crystal from its equilibrium position at the boundary through a certain angle. If W is comparable to or greater than the energy of intermolecular interactions in the liquid crystal then the cohesion is called strong; otherwise it is called weak. Owing to long-range orientational ordering (see Orientational order), the conditions of cohesion at the surface affect the bulk properties of the liquid crystal. For example, in the case of weak cohesion the threshold tension of a Frederiks transition is reduced; at the same time, the response time decreases with a simultaneous increase in the steepness of the voltage–contrast characteristic in a liquid crystal cell, and this allows one to increase the information capacity of liquid-crystal displays. Boundary effects inﬂuence not only in the type of orientation of the molecules

132

BOUND WATER

on the surface, but also the degree of order in the interior. Near the surface the degree of order differs from that in the bulk (the former being higher, as a rule). It is experimentally possible to form, at the boundary of a nematic liquid crystal, a thin layer of smectic liquid crystal that is characterized by extra translational ordering of the molecules, and by a higher degree of orientational ordering of their long axes. The spatial inhomogeneity of the degree of ordering near the liquid crystal surface results in a macroscopic electric polarization of the subsurface layer which is referred to as order electricity (compare with the exoelectric effect). BOUND WATER, combined water

Water interacting with the surface of mineral particles, and thereby acquiring some special properties. It freezes at temperatures below 0 ◦ C. The “bonding” mechanism of water in rocks involves the processes of physical and chemical adsorption, capillary condensation (see Capillary phenomena), and osmosis. The action of surface forces in minerals results in the perturbation of hydrogen bonds between the molecules of water, which is then transferred in succession from molecule to molecule of water. Bound water is usually separated into adsorbed, capillary, and osmotic types. Adsorbed water is more strongly held at the surface of minerals, and is therefore considered strongly bound, while capillary and osmotic water are both weakly bound. Strongly bound water is nonuniform. One may identify “island” water adsorption (bonding energy within 40–130 kJ/mol) and multilayer adsorption (bonding energy within 0.4–40 kJ/mol). Capillary and osmotic water are contained in rocks at humidities exceeding the maximum rock hygroscopicity. They both differ in their properties from either free or strongly bound water. Osmotic water may only be contained in rocks if some ions are present. It is the type most weakly bound to the surface, with its bonding energy remaining below 0.4 kJ/mol. The freezing temperature for capillary and osmotic water varies from −0.2 to −(2–3) ◦ C. BOUSSINESQ EQUATION (J. Boussinesq, 1871)

An equation of the form Ut t − Uxx − 6(U 2 )xx − Uxxxx = 0, where U (x, t) is the velocity ﬁeld; and x and t are, respectively, the space

and time coordinates written in a dimensionless form (subscripts denote partial differentiation). This equation was introduced by Boussinesq to describe the propagation of waves of small but ﬁnite amplitude when the dissipation is negligible, and characteristic wavelengths signiﬁcantly exceed the reservoir depth. In solid-state physics, the Boussinesq equation is also referred to as a nonlinear string equation in connection with its application to the theory of nonlinear waves of a one-dimensional lattice and a nonlinear string. The Boussinesq equation is more general than the Korteweg–de Vries equation (see Soliton) because it takes into account motion in both directions. The Boussinesq equation is completely integrable by the inverse spectral transformation associated with a scattering problem for a third order operator. Therefore, it has all attributes pertinent for integrable systems: an inﬁnite series of polynomial conservation laws, Bäcklund transformation, and many-soliton solutions. The simplest singlesoliton solution of the Boussinesq equation is x ± ct 1 2 2 , U (x, t) = c − 1 Sech 4 Δ where c is the soliton velocity, and Δ = 2(c2 − 1)−1/2 is its width. It is a single parameter family of stationary solitary waves. There are several modiﬁcations of the Boussinesq equations which cannot be integrated. In particular, Ut t − Uxx − 6(U 2 )xx − Uxxt t = 0 is the adjusted Boussinesq equation used to describe longitudinal acoustic waves in rods; and Ut t − Uxx − 6(U 3 )xx − Uxxt t = 0 is the modiﬁed adjusted Boussinesq equation used in the theory of nonlinear seismic waves. BOUSSINESQ–GALYORKIN SOLUTION (J. Boussinesq, B.G. Galyorkin)

A general solution of the equilibrium equations of an elastic medium in the absence of bulk forces expressed via an arbitrary biharmonic vector. If the equilibrium equation is written in the form (1 − 2ν)∇ 2 u + grad div u = 0, where u is the displacement vector, and ν is the Poisson ratio, then the Boussinesq–Galyorkin solution has the form: 1 (1 − ν) × grad div f , u = ∇2f − 2

BRAGG MULTIPLE SCATTERING

where f is an arbitrary biharmonic vector, i.e. a vector satisfying the equation ∇ 2 ∇ 2 f = 0. BRAGG DIFFRACTION (W.L. Bragg)

A type of diffraction of X-rays, neutrons, electrons, etc., by crystals when the reﬂection from each plane of atoms is specular, and the rays reﬂected from successive planes constructively interfere with each other. Symmetric and asymmetric Bragg diffraction are distinguished in which the reﬂecting planes (hkl) are parallel or not parallel to the entrance plane of the crystal, respectively. The most important effect in Bragg diffraction is the total interference reﬂection of the transmitted wave in a small angular interval (for X-rays, a few seconds of arc) due to the extinction effect when the wave ﬁeld penetrates a crystal to a depth of the order of the extinction length. The reﬂectivity of a crystal of ﬁnite thickness in Bragg diffraction has some subsidiary maxima in its angular dependence, which are the analogues of the pendulum solution in Laue diffraction. Bragg diffraction is mostly employed to check the structural perfection of the near-surface layers of crystals. Unlike Laue diffraction, Bragg diffraction is not limited by sample thickness t ; and for thick samples t tn , where tn is the absorption length, the diffraction pattern is simpler, and it is more readily interpreted. BRAGG DOUBLE REFLECTIONS

This diffraction occurs when an X-ray, electron, neutron, etc., beam reﬂected in accordance with the Bragg law from a family of parallel planes in a crystal reﬂects again from the planes of the same family. The direction of propagation and the intensity of Bragg double reﬂections are determined by the crystal structure of a crystal, and by the experimental conditions. While the ﬁrst and the second reﬂections occur in crystal regions disoriented by the angle δ, the direction of Bragg double reﬂections differs from that of the primary radiation by the angle ε = δ sin θ where θ is the Bragg angle. There are three kinds of Bragg double reﬂections in polycrystals: intrablock, intragrain and intergrain ones. At large scattering angles (ε 10◦ ), these reﬂections are veiled by the diffuse background due to Compton scattering (see Compton

133

effect) and thermal scattering. At small scattering angles (ε 1◦ ), the contribution of Bragg double reﬂections is signiﬁcant and exceeds the thermal and the Compton scattering by several orders of magnitude. The small-angle scattering of X-rays due to Bragg double reﬂection allows one to determine the size of grains and blocks in polycrystals, their orientation distribution, and the angular block disorientation (see Bragg multiple scattering). BRAGG LAW, Bragg relation (W.H. Bragg, W.L. Bragg, G.V. Vulf, 1913) The main equation of X-ray diffraction. X-ray

diffraction from the atomic lattice of a monocrystal can be formally described as reﬂection from atomic planes. According to the Bragg law, the angle of reﬂection (Bragg angle) θ between the atomic plane and diffracted beam satisﬁes the condition 2dhkl sin θ = nλ, where dhkl is the interplane distance between the series of parallel atomic planes with crystallographic indices (hkl), λ is the X-ray wavelength, and n = 1, 2, 3, . . . is the order of the reﬂection. BRAGG MULTIPLE SCATTERING Scattering of radiation in a crystal under the conditions when the Bragg relation (see Bragg law) is valid for two or n reﬂections simultane-

ously. One can represent the conditions of the Bragg multiple scattering with the help of an Ewald sphere in k -space: the Ewald sphere with radius |k 0 | = 1/λ corresponds to the incident radiation with wavelength λ. Vectors k 0 , k 1 , k 2 corresponding to the incident wave and waves reﬂected from reciprocal lattice sites (1) and (2) for the case of triple Bragg scattering are shown in the ﬁgure (n = 3, including the primary beam). Here, |k 0 | = |k 1 | = |k 2 |. By rotating the crystal about the scattering vector (straight line H01 connecting sites (0) and (1)), one can remove site (2) from the Ewald sphere, i.e. violate the Bragg condition for the site and thus exclude the triple dynamic scattering. At this, site (1) remains at the sphere and the Bragg condition applies to it (see Bragg double re ections). The greater the dimensions of a crystal unit cell and the shorter the wavelength λ (i.e. the larger the Ewald sphere radius),

134

BRAGG RULE

BRAKING RADIATION See Bremsstrahlung. BRANCHING OF FRACTURES

Bragg multiple scattering.

the greater the number of reciprocal lattice sites that can be on the sphere. That is, the more difﬁcult it will be to ﬁnd a position of the crystal where there is no Bragg multiple scattering. The evaluation of the contribution of the Bragg multiple scattering to the intensity of the measured reﬂection is quite a difﬁcult problem to solve, considering that it is complicated by the crystal mosaicity, the divergence, and the nonmonochromaticity of the incident radiation. Bragg multiple scattering allows one to observe reﬂections in those directions where the Bragg scattering is prohibited by the crystal symmetry conditions; this is the so-called Renninger effect (M. Renninger, 1937). Bragg multiple scattering in crystals can also play a positive role, e.g., it underlies one of the methods of high-precision determination of crystal lattice parameters. BRAGG RULE

This rule involves charged particle energy loss during the passage through a material with the chemical formula Al Bm Cn . . . and it is expressed by the approximate relation dE dE dE +m − =l − − dZ dZ A dZ B dE +n − + ···, dZ C where (−dE/dZ)i , i = A, B, C, are the energy losses per unit length due to the ith component of the material.

A process of the separation (bifurcation or polyfurcation) of a main-line fracture into two or more secondary ones. One can distinguish quasistatic branching of fractures caused, in particular, by processes of plastic deformation at its vertex, and dynamic branching which is observed when the fracture attains about 60% of the speed of transverse elastic waves. Due to this the stresses in front of the fast moving fracture stop being a maximum, and the failure becomes more probable in other directions. Dynamic branching of fractures has been observed in hardened glasses (see Vitreous state of matter), steels, Plexiglas and epoxy resins. Branching arises in the core layers of a sample at the front of the main-line fracture, and is directed along the tangent to the curved segment of the fracture trajectory. Thus, a secondary fracture is oriented at an angle of approximately 30◦ with respect to the primary one. After each act of branching the speed of the main-line fracture decreases. Therefore, multiple branching produces destructions that move in jumps with high accelerations, up to 108 m/s2 , thus managing to branch at small distances (e.g., in the millimeter range for hardened steel), break loose, pick up critical speed, and then branch again. The branching is stimulated by internal residual stresses that arise in the sample being fractured. BRASS

Alloy of copper and zinc belonging to the class of compounds with metallic bonding. It exists over a wide range of concentration. At low Zn content the alpha phase (face-centered cubic lattice) is formed. At higher Zn content the stability of the new phases (the so-called “electronic phases”) is determined by the average concentration n of valence electrons per atom via the proper matching of the Fermi surface and the Brillouin zone. The three electronic phases are the beta phase (compound CuZn, body-centered lattice, n = 3/2, below 460 ◦ C ordered according to the CsCl type), gamma phase (compound Cu3 Zn8 , complex cubic lattice, ordered, contains 52 atoms, n = 21/13) and epsilon phase (compound CuZn3 , hexagonal

BREAKDOWN

135

Brass phase diagram.

close-packed lattice, n = 7/4). Unusual mechanical properties are found in β-brass, caused by a martensitic transformation (shape memory effect, superelasticity, high damping). The ﬁgure shows the phase diagram. BRAVAIS LATTICES (A. Bravais, 1848)

The classiﬁcation of three-dimensional lattices into 14 types that takes into account the full point symmetry groups (holohedries) and the parallel translation groups. If a Bravais coordinate system (chosen along the most symmetrical directions of the lattice) coincides with the principal lattice system then the Bravais parallelepiped constructed on it contains lattice sites only at its apices, i.e. is a primitive parallelepiped. Such lattices are called primitive or P lattices; all other lattices are referred to as centered lattices. There are three ways to center the Bravais parallelepipeds, I – body-centered, F – facecentered, and C – base (or side)-centered. Two lat-

tices are included in the same Bravais type if their coordinates are the same and the parallelepipeds are centered identically. The Bravais classiﬁcation has also a group theory basis: two lattices are included in the same Bravais type if their full symmetry groups are isomorphous (see Isomorphism). These groups (14 out of 73 symmorphic space groups) are called Bravais groups and are designated by the symbols of the space groups. Each of 14 Bravais types is presented in Table 1 (see next page) by a corresponding Bravais parallelepiped with points at the apices, and where appropriate, with centering points indicated (see inside front cover). BREAKDOWN of solids

A sharp increase of electric current density in insulators and semiconductors that occurs when a

certain critical level of the applied electric ﬁeld strength, Ecrit , is reached. The value Ecrit is called the electric strength. The value of Ecrit falls within

136

BREAKDOWN Table 1. Bravais lattices Lattice type System

Primitive

Base-centered

Body-centered

Face-centered

Triclinic

Monoclinic

Orthorhombic

Trigonal (rhombohedral)

Tetragonal

Hexagonal

Cubic

105 –107 V/cm for various dielectrics and starts from 105 V/cm for semiconductors. During impact ionization it may be as low as 1 to 10 V/cm. One may distinguish between the electric and thermal mechanisms of breakdown. The mechanism of electric breakdown is typically characterized by an avalanche increase of the number of free carriers (electrons or electron–hole pairs), for example due to ionization by collision. Current lamentation may also occur, i.e. a conducting channel in which the current density is higher than its average across the sample may form. This effect results from an instability of the spatially homogeneous distribution of carriers when the sample

current–voltage characteristic has an S-shape. In

the case of an electric breakdown the value of Ecrit only weakly depends on the sample temperature, thickness, and the duration of electric ﬁeld pulse, τ , provided τ = 10−7 –10−6 s. Thermal breakdown results from melting of the material via Joule heating when its thermal equilibrium is disturbed (thermal breakdown without a disturbance of thermal equilibrium is also known, the so-called type II thermal breakdown). A combined mechanism of breakdown is possible, when the Joule heating of a particular region of the sample works to lower the value of Ecrit necessary for an electrical breakdown in that region. The application of a strong

BREMSSTRAHLUNG

137

ﬁeld may result in a gradual change of the composition and structure of an insulator, so that both eventually work to lower the value of Ecrit . These effects could, for example, lead to the formation of color centers in alkali-halide crystals or to erosion of polymer surfaces. Such processes are called electric aging of insulators. In contrast, dielectric breakdown in semiconductors may not necessarily be accompanied by changes in the crystal lattice. In certain cases, when the conduction electron concentration is limited and the ﬁeld strength, E is moderate, the initial process of breakdown does not result in the failure of the material, and may be repeatedly reproduced (see Impurity breakdown, Thermoelectric instability of photocurrent, Streamer breakdown). For different varieties, see also Acoustic breakdown, Electric breakdown, Magnetic breakdown.

more parts. Breaking stress is deﬁned by the ratio of the load to the specimen cross-section at the moment of failure. In brittle metals (see Alloy brittleness) this stress is achieved via the opening of brittle cracks when the external stress remains below the yield limit, and macroscopic plastic deformation is absent. When plastic metals subjected to stresses exceed the yield limit, there develops a tough failure or a quasi-brittle failure in them, while the failure stress exceeds the yield limit because of strain hardening. Failure stress in brittle metals depends only weakly on the temperature, approximately as the elastic modulus, while its dependence in plastic materials is controlled mainly by the temperature dependence of the yield limit, and may happen to be stronger.

BREAKDOWN NOISE See Telegraph noise.

An exact solution of the secular equation for the spin Hamiltonian of a paramagnetic ion with electron effective spin S = 1/2, nuclear spin I , and isotropic g, g n and hyperﬁne (A) tensors. The energy levels are as follows:

BREAKING STRAIN Strain that results in the break-up of a body into several macroscopic parts (failure). The break-

ing strain produces such a degree of deformation that it results in failure. This strain is one of the principal characteristics of a material, delimiting its margin of plasticity. It is determined during the mechanical testing of materials. Breaking strain depends on the type of state of stress (distension, compression, e xure etc.), i.e. on the “rigidity” of various types of mechanical n , tests, and on the softness factor a = tmax /Smax which is the ratio of the maximum tangential tension, tmax to the maximum normal reduced stress, n . With an increase in the material capabilSmax ity to withstand stress the plastic deformation increases. Breaking strain also depends on the type of crystal lattice, the structure, testing temperature, environment, etc. When determining the level of breaking strain the scheme reproducing both the tensed and the deformed states of the specimen during tests should be as close as possible to the actual operating conditions of the material. BREAKING STRESS, failure stress, failing stress

A stress reached during distension tests, which result in the breakup of the specimen into two or

BREIT–RABI FORMULA (G. Breit, I. Rabi)

Δ − gn βn BmF 2(2I + 1) 1 4xmF 1/2 ± Δ 1 + x2 + , 2 2I + 1

E(F, mF ) = −

where F = I + 1/2, mF = m ± 1/2, m = −I, . . . , +I ; Δ = a(I + 1/2) is the splitting in zero magnetic ﬁeld B; a is the isotropic hyper ne interaction constant, x = (gβ + gn βn )B/Δ, and β and βn are the Bohr and nuclear magnetons, respectively. BREMSSTRAHLUNG, braking radiation, collision radiation

An emission of photons by electrically charged particles decelerating in an electric ﬁeld (or in a magnetic ﬁeld, called magnetic Bremsstrahlung or synchrotron radiation). The intensity of Bremsstrahlung is proportional to the square of the particle acceleration, i.e. proportional to Z 2 /M 2 where Z is the atomic number, and M is the mass of the nucleus being decelerated by the electric ﬁeld. Owing to the small mass of elec-

138

BREMSSTRAHLUNG, COHERENT

trons and positrons, the intensity of their Bremsstrahlung is 3·106 times greater than that for protons. This leads to a substantial contribution to the Bremsstrahlung by the energy loss of fast electrons and positrons in a medium (see Charged particle energy loss). The spectrum of Bremsstrahlung is continuous. The maximum value of the energy of the emitted photon is ωM = E − mc2 (here E is the total energy, m is the electron mass, and c is the speed of light). In a crystal the constructive interference of photons scattered by closely situated atoms of the crystal inﬂuences some speciﬁc features of the Bremsstrahlung, in particular the intensity of the Bremsstrahlung increases (see Coherent Bremsstrahlung). These changes are especially signiﬁcant in the case of the channeling of electrons and positrons (see Quasi-characteristic radiation). See also Radiation by charged particles. BREMSSTRAHLUNG, COHERENT

See Coherent Bremsstrahlung. BRILLOUIN FUNCTION (L. Brillouin, 1926)

Function Bj (x) introduced to describe paramagnetism of noninteracting atoms. For atoms with the angular momentum j (in units of Planck constant ), the function is Bj (x) =

2j + 1 2j + 1 coth x 2j 2j −

1 x . coth 2j 2j

The Brillouin function determines the mean value of the projection of j on the direction of the magnetic ﬁeld H (directed along the z axis) jz = j Bj (x), x = gj |μB |H /(k B T ), where μB is the Bohr magneton and gj is the Landé g -factor. The Brillouin function is the basis for the quantum theory of paramagnetism of substances with uncompensated atomic magnetic moments, and of magnetically ordered materials (when described in the framework of the molecular eld approximation; in this case, H is the effective magnetic ﬁeld).

BRILLOUIN SCATTERING, also called Mandelshtam–Brillouin scattering Inelastic light scattering by thermal acoustic phonons in condensed media with the light fre-

quency changed by a value equal to a phonon frequency. (Analogous processes by optical phonons are called Raman scattering of light). The scattering is caused by ﬂuctuating inhomogeneities of the refractive index, which are related to propagation of thermal (Debye) excitations of a medium. From the classical point of view, Brillouin scattering can be interpreted as result of the diffraction of light by thermal elastic waves. By virtue of the diffracted light interference, only waves with wavelength Λ, which satisﬁes the Bragg condition λl = 2nΛ sin(θ/2) (where n is the refractive index of the medium, λl is wavelength in vacuum, θ is angle of scattering), are responsible for scattering in a given direction. Furthermore, due to the Doppler effect, the light with frequency ωl , which is scattered by elastic waves, undergoes a frequency change ωs = ωl ± ω0 , deﬁned by the relationship ω0 /ωl = ±v/(Λωl ) = ±2n(v/c) sin(θ/2), where c is the speed of light in vacuo, and v is the sound velocity in the medium. Elastic waves with frequency ∼1010 Hz (hypersonic waves) are of importance in the light scattering. The line width is determined by hypersound attenuation. The scattering efﬁciency is of the order of 10−6 scattered photons per incident photon. However, if the intensity of the incident light exceeds some threshold value (∼1010 W/cm2 ), an avalanche-like growth of the amplitudes of sound and of scattered waves occurs, a process called stimulated Brillouin scattering. Brillouin scattering is used for studying material properties: sound wave propagation velocity and decay rate, molecular structure, intermolecular interactions, etc. Stimulated Brillouin scattering is used for the generation of intense hypersonic waves, and in experiments on wave front reversal of light waves. Resonance Brillouin scattering is an effective method for investigating excitonic polaritons. BRILLOUIN ZONE

A limited region in the reciprocal space (k -space) of wave vectors inside which the quasiparticle energies in the crystal take on the entire

BRITTLE FRACTURE

spectrum of permitted values. The overall k-space can be partitioned into an inﬁnite number of Brillouin zones of the same dimensions, and equal in volume to a reciprocal lattice cell. The use of a single Brillouin zone is due to the crystal periodicity since the quasi-particle energy E(k) is periodic in the quasi-momentum space with the periodicity of a reciprocal lattice vector G: E(k) = E(k + G). A region with its center at the point k = 0 is chosen as the ﬁrst Brillouin zone, or simply referred to as the Brillouin zone. It is delimited by planes passing through the mid-points of the lines (normally to them) that connect point k = 0 with neighboring sites of the reciprocal lattice. A Brillouin zone is analogous to a Wigner–Seitz cell in real (coordinate) space. Its boundaries are determined by the reciprocal space form of the Bragg equation 2k·G = G2 , involving a reciprocal lattice vector. At the boundaries the quasi-particle energy E(k) reaches an extremum. To describe some physical phenomena it is convenient to use the extended Brillouin zone scheme which makes use of the periodicity of the quasi-particle spectrum in k-space. BRITTLE CRACK A crack, whose propagation is not followed by a plastic deformation. During brittle crack propagation the theoretical strength is reached at its

vertex. The breaking of interatomic bonds occurs without activation. Elastic energy, stored in the material during a deformation process, converts into surface energy at its propagation. The critical stress for the brittle crack propagation is determined by the Grifﬁth equation (see Grif th theory). BRITTLE FAILURE

A type of solid failure involving purely elastic strains. Ideally only materials with no capability for plastic deformation (e.g., glass, ceramics, diamonds, some minerals) undergo brittle failure under conditions of ordinary tension. Metals, due to the presence of dislocations, behave as ideally brittle only in special circumstances when the failure is initiated in extremely small regions. These regions have an ideal (defect free) structure in perfect crystals (whiskers), or in microregions near the tip of atomically-sharp submicrocracks,

139

where a fracture of atomic bonds occurs through microspalling (without attendant plastic deformation). However, in so far as the origin of microcracks in metals is possible only as a result of the displacement and pile-up of dislocations, so a failure in metallic materials can only be of a quasibrittle type (see Quasi-brittle failure) since a condition of purely elastic deformation does not appear at their failure. In practice when a failure of products, constructions and installations (e.g., hulls of ships) occurs, it is considered to be the brittle type, if an overall deformation of the product was elastic before its failure, in spite of the fact that a large local plastic deformation took place in the focus of failure. Hence in practice the term “brittle failure” does not have a precise meaning. However, it can correspond to a complicated type of failure combining features of overall elastic and local plastic deformation. The latter forms only in small regions near cracks, or in action zones of large residual stresses of a welding or quenching origin. An important feature of such a failure is that the average (nominal) failure stress should be less than the yield limit of the material. Excessively high strength of the material, low temperature (cold brittleness), high velocity of deforming (a shock load), the presence of cracks or other concentrators of stresses, the presence of large residual macrostresses of the ﬁrst type; all of these factors contribute to the signiﬁcance of brittleness in engineering practice. BRITTLE FRACTURE A fracture arising from brittle failure. This type of failure is associated with failure by spalling,

when a progression of the crack is not accompanied by plastic deformation, and failure occurs over the plane of crystal cleavage through the breaking of atomic bonds. Actual brittle failure has been found in covalent crystals such as diamond and silicon carbide. A brittle transcrystalline failure is possible also in other crystals with a high degree of covalent bonding, where dislocations are practically “frozen in”. The typical feature appearing on the surface of a brittle fracture is a step of spalling arising at the intersection of a screw dislocation and a crack front. A junction of the splitting steps makes up a stream-like pattern. The same

140

BRITTLENESS AND TOUGHNESS CRITERION

features of fracture are typical for quasi-brittle failure through splitting accompanied by plastic deformation of the region adjacent to the crack. Such a failure is typical for crystals with body centered cubic lattices at ambient temperatures. Intercrystalline brittle failure occurs at sharply weakened intergranular linkages. It is observed along grain boundaries through the catastrophic crack progress due to the segregation of impurities, and also to the presence of internal stresses. Intercrystalline failures along boundaries of grains and subgrains are distinguished. When a failure runs along grain boundaries a fracture is completely free from a stream-like pattern, linkage points of three (or more) boundaries of grains appear, and often a “bubble” due to the segregation of impurities is observed on facets of split grains.

the failure is supposed to be tough. In mechanics, the engineering criterion of brittleness is used, whether the product is destroyed by the average (nominal) stress σn below the yield limit σy , i.e. when σn < σy , which can be satisﬁed only in the presence of stress concentrators (see Stress concentration). BRITTLENESS, BLUE See Blue brittleness. BRITTLENESS OF ALLOYS See Alloy brittleness. BROADENING OF A LINE See Line (level) width. BROKEN BOND The same as Dangling bond.

BRITTLENESS AND TOUGHNESS CRITERION

This is a condition determining the relation of parameters responsible for the type of failure of a solid under load. There is no unique brittleness and toughness criterion, since these criteria differ in various areas of science involving failure problems. In solid state physics, the brittleness and toughness criterion is connected with the possibility of plastic stress relaxation via the generation of dislocations by a vertex of a perfectly sharp crack in a crystal. This possibility depends on the relation between theoretical strength against shear τtheor and rupture σtheor and maximum tangential τmax and tensile stress σmax at the vertex of the crack. If τtheor /σtheor < τmax /σmax , the crystal is tough (FCC metals: copper, silver, gold); otherwise, it is brittle (diamond and BCC metals: tungsten, iron, sodium). In physical materials science, as a brittleness and toughness criterion, the one based on the microspalling criterion my be chosen: if j > Kt , then the failure is brittle, if j < Kt , then it is tough (more precisely, a quasibrittle failure). According to the fractographic classiﬁcation of destruction types, one does not succeed in giving a clear distinction between brittleness and toughness in metals, and brittleness and toughness criteria are qualitative: if in a fracture of brilliant facets of a spalling no appreciable traces of plastic deformation are seen, then the failure is supposed to be of a brittle (or quasi-brittle) type; if typical pores or pits are observed (a ﬁbrous break),

BROOKS–HERRING FORMULA (H. Brooks, C. Herring)

This expression determines the energy dependence of the mean free path time τ (E) of charge carriers of energy E in semiconductors when the scattering takes place predominantly from ionized impurities (low temperatures, high impurity concentrations). The Brooks–Herring formula is τ (E) =

ε2 (2m∗ E 3 )1/2 , πe4 NΦ(x)

where ε is the dimensionless dielectric constant; m∗ is the effective mass of the carriers, N is the impurity concentration, Φ(x) = ln(1 + x) − x/(1 + x) where x = 8m∗ E/(2 q 2 ), q is the inverse Debye screening radius. It follows from the Brooks–Herring formula that scattering by ionized impurities becomes more efﬁcient at small carrier energies and, consequently, at low temperatures. The Brooks–Herring formula was derived in the Born approximation of collision theory taking into account the screening of impurities by free carriers. In its derivation the impurities are assumed to be arranged in a crystal lattice in a disordered way (see Current carrier scattering). BUBBLE DOMAIN See Magnetic bubble domain. BUBBLE DOMAIN LATTICE See Magnetic bubble domain lattice.

BULK PHOTOVOLTAIC EFFECT

BUCKYBALL See Fullerene. BULK ACOUSTIC WAVES Propagating periodic strains of an elastic me-

dium obeying the wave equation ρ∂ 2 ui /∂t 2 − cij kl ∂ 2 uk /∂xj ∂xl = fi , where ρ is the medium density, u is the displacement of the medium element, cij kl are the components of the elastic modulus tensor, and f is the bulk density of the external (nonelastic) forces. In contrast to liquids and gases, solids can support the propagation of traverse waves in addition to longitudinal waves; the displacements in the former being normal to the propagation direction. Three natural modes of acoustic waves exist in an isotropic body (see Isotropy): one longitudinal acoustic wave with the velocity v = (c1111 /ρ)1/2 , and two degenerate transverse acoustic waves with v⊥ = (c1212 /ρ)1/2 . In an anisotropic medium (such as a crystal) pure longitudinal and traverse waves can propagate only in preferred directions which have sufﬁciently high symmetry. For an arbitrary propagation direction, there are three modes of bulk waves with different phase velocities (a typical sound velocity in solids is v ≈ 105 cm/s). Acoustic waves can be classiﬁed by their frequency. Waves in the audible and infrasonic range (f < 104 Hz) lack important applications in solid state physics due to their long wavelength. Waves with frequencies from 20 kHz to 1 GHz are called ultrasonic (ultrasound), and are widely used in physics and engineering. The frequency range 109 to 1012 Hz, called hypersonic (hypersound), exhibits quite sizable attenuation (attenuation coefﬁcient κ > 1 cm−1 ). Acoustic waves with frequencies above 1012 Hz are called terasound, and exhibit a signiﬁcant dispersion as their wavelength becomes comparable to the crystal lattice period. Sound velocity dispersion and anisotropy of the medium cause the group velocity characterizing the propagation of perturbation waves, which has a narrow spectral-angular distribution (v gr = ∂ω/∂k), to differ from the phase velocity describing the phase propagation (v ph = kω/k 2 ) in both magnitude and direction. BULK CHARGE The same as Space charge.

141

BULK FORCE, volume force

A force distributed over the volume of a material. It is characterized by a volume force density f , i.e. a force acting upon a unit body volume. An example is a mass force f that acts on mass and is associated with the acceleration a of a body: f = −ρa, where the density ρ can depend on the position, and vary throughout the body. The force of gravity f G (at the Earth’s surface f G = ρg, where g is the acceleration of gravity) is a special case of a mass force. Other volume forces are: a thermoelastic force (see Elasticity theory, Thermoelasticity); the forces of electric and magnetic ﬁelds acting upon charges and magnetic moments, respectively; and the force acting upon the body from the conduction electrons that drift in an electric ﬁeld E, f = enE (here n is the number of conduction electrons per unit volume, e is the electron charge). BULK MODULUS, compressibility modulus One of the elastic moduli of an isotropic medium, K; it is expressed via the Lamé coef cients

as K = λ + (2/3)μ. Its reciprocal value is called the compressibility. In crystals of cubic symmetry, K = (c11 + 2c12 )/3 (here cik are the secondorder elastic moduli in Voigt notation). The bulk modulus is measured in pascals. K is 0.77 GPa for Al; 1.37 for Cu; 1.78 for Fe; 0.75 for Ge; 0.24 for NaCl; 4.00 for diamond. BULK PHOTOVOLTAIC EFFECT

The appearance of a stationary photocurrent under uniform illumination of a macroscopically homogeneous piezoelectric (see Piezoelectricity) or ferroelectric crystal. A bulk photovoltaic effect was discovered in the late 1960s which exhibited a linear dependence of the photocurrent on the light intensity (see Glass’ constant). The effect leads to the generation of photoelectric voltages which can exceed the band gap width by several orders of magnitude, and are limited only by the photoconductivity of the crystal. The direction and magnitude of the photocurrent depend on the orientation of the light polarization. Linear and circular effects are known. Phenomenologically, it is convenient to establish the characteristics of the bulk photovoltaic effect by expanding the photocurrent Ii in a power series of the electric ﬁeld Ej as Ii = σij Ej + αij k Ej Ek∗ + γij i EE ∗ j + · · ·

142

BULK SOUND HARDENING

The ﬁrst term with the second-rank tensor σij describes photoconductivity in an external ﬁeld Ej . The second term describes the linear bulk photovoltaic effect (i.e. in linearly polarized light); Ej and Ek being the projections of the light polarization vector. The components of the third-rank tensor αij k of this effect differ from zero for only 20 piezoelectric symmetry groups. The third term describes the circular photovoltaic effect. The microscopic theory of the bulk photovoltaic effect takes into account two basic mechanisms. The ﬁrst, so-called ballistic, mechanism is related to the asymmetry of the distribution function of the nonequilibrium carriers in momentum space. This asymmetry, in its turn, is caused by the asymmetry of the generation, recombination, and scattering of the nonequilibrium carriers in a crystal without a center of symmetry. The second, so-called shift mechanism, is due to displacement of the center of gravity of the wave packet of an electron during its optical transition between bands, or between an impurity center and a band in a crystal without a center of symmetry. The two mechanisms describe both intrinsic and impurity bulk photovoltaic effects, and predict similar magnitudes of the bulk photovoltaic effect. Therefore, the experimental differentiation of these mechanisms is a complicated task. At present, the linear and circular effects are observable in a large number of ferro- and piezoelectric crystals, including ferroelectric niobates and tantalates, Te, GaAs, GaP, ZnS, and some other piezosemiconductors.

can control processes of homogenization, recovery, recrystallization, and phase transitions. A speciﬁc feature of the action of intensive vibrations on a material is the nucleation and growth of microcracks (see Crack) at early stages of loading, a fatigue type phenomenon. Depending on the conditions of treatment, and the initial state of materials, acoustic dehardening may occur, e.g., with sound waves incident on initially deformed metals with a face-centered cubic lattice. BURGERS CONTOUR

A contour constructed in a regular crystal lattice by sequentially tracing a closed line from one atom to another. It is used to classify defects in crystals, and is of particular importance for the description of linear defects or dislocations (Fig. (a)). If a dislocation appears in a crystal enclosed with such a contour, the contour remains open. In order to close a Burgers contour, it must be complemented with a vector called a Burgers vector that closes the break (Fig. (b)). A Burgers vector b characterizes a dislocation unambiguously. Linear needle-shaped defects of different types unconnected with translational slip of a part of a crystal

BULK SOUND HARDENING, sonic strengthening An increase of the yield limit, microhardness

and other mechanical properties, observable during propagation of high-intensity elastic waves (sonic waves) in solids, mainly in metals. For every material in equilibrium there is a critical vibration amplitude, which depends on the ambient temperature and frequency. It is starting from this amplitude that the density of dislocations, vacancies and other defects of the crystal structure increases. The shape and the size of a mechanical part remains practically unchanged in this case, which is an advantage of this method of hardening (see Strain hardening). Bulk sound hardening can arise due to the intensiﬁcation of thermally activated processes. Using the latter, one

Burgers contour in a defect-free crystal (a) and in a crystal with an edge dislocation (b). In the latter case, the Burgers contour is closed with the Burgers vector b.

BURSTEIN–MOSS EFFECT

relative to another part (chain of vacancies, chain of impurity atoms, etc.) never cause a break of a Burgers contour. Sometimes a closed Burgers contour is constructed within a crystal with a dislocation (Burgers contour in the Frank interpretation). Then, upon removal of the dislocation from the crystal, the Burgers contour turns out to be open, and it is closed by a Burgers vector. When dealing with small-angle and large-angle grain boundaries, use is also made of a special Burgers vector constructed in the reference lattice (contour in Frank’s interpretation). This contour is constructed with the help of similar (according to the crystallographic direction) vectors drawn in neighboring grains so that the vectors originate from the same point located at the boundary. The Burgers contour is closed in this case with the closure vector B. BURGERS EQUATION (J.M. Burgers, 1940)

An equation of the form Ut + U Ux − μUxx = 0, where U (x, t) is the velocity ﬁeld; x, t are space and time coordinates, subscripts indicate partial differentiation, and μ is the viscosity coefﬁcient. The equation is a one-dimensional reduction of the Navier–Stokes equations (see Continuum mechanics), and is the simplest member from among the most important equations of the physics of nonlinear waves. Burgers equation gives a good description of the dynamics of weakly nonlinear waves in continua, including solids, when only ﬁrst order dissipation effects are taken into account. The complete solution of Burgers equation is connected with the Cole–Hopf transformation (J.D. Cole, 1951; E. Hopf, 1950): U = −2μ(ln ϕ)x , which transforms the former into the linear diffusion equation: ϕt − μϕxx = 0. If there is no dissipation (μ = 0), then the nonlinearity causes a gradual increase of the wave front slope, and ﬁnally leads to the formation of a break (simple Riemann wave). The latter, increasing in the presence of viscosity (μ > 0), leads to the intensiﬁcation of dissipation effects that seek to decrease the proﬁle slope. It is the mutual compensation of these contradicting trends, represented in Burgers equation by the last two terms, that brings about the possibility of the propagation of waves with a stationary proﬁle, including a shock wave with a ﬁnite shock width, directly propor-

143

Closed dislocation line in a crystal: A is the region unaffected by the shift; B is the region where a shear deformation has occurred; Burgers vector b is indicated.

tional to μ and inversely proportional to the shock amplitude. BURGERS VECTOR (J.M. Burgers, 1939)

The most important translational characteristic of linear defects in crystals is the Burgers vector (b) which closes an open Burgers contour around a dislocation line. When there is no dislocation, the contour is closed. The magnitude and direction of a Burgers vector determine how a portion of material on one side of the dislocation line is shifted relative to the material on the other side (see Fig.). A Burgers vector and a tangent vector of the dislocation line determine the slip plane of a dislocation element. In magnitude, a Burgers vector can equal either a whole repetition period of the crystal lattice in the vector direction (for perfect dislocations) or equal a fractional part of it (for partial dislocations). A Burgers vector is constant along the entire length of a dislocation line, whatever its conﬁguration, and remains constant during the dislocation motion. The sum of Burgers vectors of dislocations meeting at a dislocation site equals zero if all the dislocation lines are directed either to or from the site (Frank networks). Elastic strains and stresses produced by a dislocation in a crystal are proportional to the magnitude of the Burgers vector, while the strain energy is proportional to its magnitude squared. When dealing with smallangle and wide-angle grain boundaries in crystals, a closure vector B is introduced, which is similar to a Burgers vector and is caused by the presence of dislocations at the boundary. This vector carries the information on the angle of disorientation of neighboring grains. BURSTEIN–MOSS EFFECT (E. Burstein, T.S. Moss, 1954) An upward shift in energy of the intrinsic light absorption edge in semiconductors accompanying

144

BURSTING

an increase of the free current carrier concentration. The Burstein–Moss effect is due to ﬁlling the bottom of the conduction band by electrons in n-type semiconductors or the top of the valence band by holes in p-type semiconductors. Then, only states above the Fermi level E F are available for transitions involving photoexcited carriers. As a result, direct optical band-to-band transitions at T = 0 K are possible with the energy of quanta satisfying the inequality 2 kF2 mn 1 + , ω ωmin = Eg + 2mn mp

where E g is the band gap, mn and mp are the effective masses of the electron and the hole, respectively; and k F is the wave vector corresponding to the Fermi level. At T > 0 K and mn /mp 1, the magnitude of the Burstein–Moss effect is approximately equal to Δω = E F −4k B T in directgap semiconductors, and in semiconductors with small mn (e.g., InSb), it already appears at carrier concentrations 1017 cm−3 . The Burstein–Moss effect is used in studies of the energy band structure of semiconductors. BURSTING See Penetration deformation.

Cc in cadmium polycrystal at T melting is 1.7·10−12 m2 /s. Effective high-energy (3 to 10 MeV) neutron cross-section for absorption and scattering is 4.3 barn, and 2610 barn for thermal (0.025 eV) neutrons. Ion-plasma frequency is 8.54 THz; lowtemperature linear electronic speciﬁc heat (Sommerfeld coefﬁcient) is 0.70 mJ·mole−1 ·K2 ; electrical resistivity is 83.6 n·m (at 293 K) along the principal axis 6 of a monocrystal and 68.7 n·m in a perpendicular direction at room temperature, thermal coefﬁcient of electrical resistance in these directions is 0.0041 and 0.00405 K−1 , respectively; Hall constant is ∼ = + 5.7·10−11 m3 /C at room temperature. Work function of cadmium polycrystal is 4.1 eV. Critical temperature of cadmium transition to the superconducting state is 0.517 K; critical magnetic ﬁeld is 2.8 mT (at 0 K). Cadmium is a diamagnetic material with molar magnetic susceptibility −19.7 · 10−6 CGS units (at 300 K); nuclear magnetic moment of 111 Cd isotope is −0.592 nuclear magnetons. Cadmium is used in nuclear power engineering and as a component of alloys for solders, printing blocks, jewelry, electrodes.

CADMIUM, Cd

Chemical element of Group II of the periodic system with atomic number 48 and atomic mass 112.41. Natural cadmium consists of stable isotopes with mass numbers: 106 (1.215%), 108 (0.875%), 110 (12.39%), 111 (12.75%), 112 (24.07%), 113 (12.26%), 114 (28.86%), 116 (7.58%). The electronic conﬁguration of the outer shells is 4d 10 5s 2 . Successive ionization energies are 8.994, 16.908 eV. Atomic radius is 0.148 nm; radius of Cd2+ ion is 0.097 nm. Oxidation state is +2. Electronegativity is ∼ =1.5. In free form, cadmium is a silvery-white forgeable and ductile metal. It has a hexagonal closepacked crystal lattice; a = 0.297912 nm, c = 0.561827 nm (at 298 K). Density is 8.65 g/cm3 at 293 K; T melting = 594 K; T boiling = 1030 K. Bond energy is 1.16 eV/atom at 0 K. Heat of melting is 6.38 kJ/mole; heat of sublimation is 112.2 kJ/mole; heat of evaporation is 99.9 kJ/mole; speciﬁc heat is 0.231 kJ·kg−1 ·K−1 ; Debye temperature is ∼ =200 K; coefﬁcient of the linear thermal expansion of cadmium monocrystal is 54.0·10−6 K−1 along the principal axis 6 and +19.6·10−6 K−1 perpendicular to it (at 300 K); coefﬁcient of thermal conductivity is 83.7 W·m−1 ·K−1 along the principal axis 6 and 105 W·m−1 ·K−1 perpendicular to it (at room temperature). Adiabatic coefﬁcients of elastic rigidity of cadmium monocrystal: c11 = 114.5, c12 = 39.5, c13 = 39.9, c33 = 50.85, c44 = 19.85 (in GPa) at 300 K; bulk modulus is ∼ =58 GPa; Young’s modulus is ∼ =65 GPa; shear modulus is ∼ =25 GPa; Poisson ratio is ∼ =0.31 (at 300 K), ultimate tensile strength is ∼ =0.08 GPa and relative elongation is ∼ =32%. Brinell hardness is ∼ =0.18 GPa. Cadmium is easily forged and rolled. Surface tension of liquid cadmium is 0.628 J/m2 (at 623 K). Self-diffusion coefﬁcient of atoms

CADMIUM SULFIDE

A semiconductor compound of the AII BVI group (see Semiconductor materials), which crystallizes in the cubic sphalerite structure (zinc ¯ blend structure), space group F 43m (Td2 ), and in the hexagonal wurtzite structure, space group 4 ). The unit cell of sphalerite P 63 mc (C6v contains four molecules with lattice parameter a = 0.5835 nm, while that of wurtzite contains two molecules, with lattice parameters a = 0.41368 nm, c = 0.6713 nm, and the ratio of anion and cation radii is 0.52. For both structures the tetrahedral positions of the atoms is characteristic, the crystals have no center of symmetry, 145

146

CALAMITICS

they are polar; they form polytypes (see Polytypism) as derivatives of basic structures. Below the pressure 3 GPa a transition to the structure of sodium chloride is observed. The cubic modiﬁcation is stable at considerably lower temperatures than those of growing monocrystals. Data given for the hexagonal wurtzite modiﬁcation are as follows: temperature coefﬁcients of linear expansion with temperature reduction from 600 to 150 K are reduced from 5.9·10−6 to 0.5·10−6 K−1 , density is 4.825 g/cm3 , melting temperature is 1748 K, heat of formation ◦ = −157 kJ·mole−1 , standard entropy

Hf,298.15

◦ = 71 J·mole−1 ·K−1 , speciﬁc heat S298.15 ◦ Cp,298.15 = 47.4 J ·mole−1 ·K−1 , heat conduc-

tivity 0.20 W·cm−1 ·K−1 , Debye temperature is 219.3 K. Covalent bonding prevails with some admixture of ionic bonding. The phonon spectrum has nine optical and three acoustic branches. The band gaps are direct, the valence band presents three closely located subbands: Γ9 (the upper one), Γ8 , Γ7 ; the ﬁnal conduction band has symmetry Γ7 . The band gap width: Eg,1.8 K = 2.58 eV, Eg,300 K = 2.53 eV. Average values of temperature coefﬁcient of Eg variation at constant pressure (dEg /dT )P in the range 90 to 300 K and coefﬁcient (dEg /dP ): −5.2·10−4 eV/K and 3.3·10−6 eV/bar. The spin– orbit interaction constant is 0.065 eV, the valence band splitting due to the crystal e ld action is 0.027 eV, electron af nity is 4.73 eV, work function is 7.26 eV. Effective masses of electrons, holes: m∗n = 0.205, m∗p = 0.7 (⊥ c), m∗p = 5 ( c). Refraction index dispersion and birefringence are characterized by the values: ne = 2.726, no = 2.743 at λ = 515 nm; ne = 2.312, no = 2.996 at λ = 1500 nm. Static and high-frequency dielectric constants are: εs = 8.64 ( c), εs = 8.28 (⊥ c), ε∞ = 5.24. The Cd–S system in the phase equilibrium diagram has one compound CdS with a narrow range of homogeneity. Inherent atomic defects to a large extent determine the diffusion and solubility of impurities, the structure of local centers, optical and electric properties. Elements of Group III Al, Ga, In, can replace the cations, elements of Group VII Cl, Br, I, replace the anions, vacancies of anions, interstitial cations are shallow hydrogen-like

donors; elements of Group I Cu, Ag, replace the cations, cation vacancies behave as deep acceptors. The association of the point defects is characteristic. Conductivity may change from a semimetal to insulator type, no p-type conductivity is observed due to the self-compensation phenomenon. Mobility of electrons and holes: 350 cm2 ·W−1 ·s−1 and 30 cm2 ·W−1 ·s−1 . Minority carrier lifetimes (holes) are 10−6 to 10−8 s, diffusion lengths of holes are short (7 to 0.5 μm). The presence of direct band gaps facilitates effective luminescent and laser radiation. Blue radiation is caused by the annihilation of free and associated excitons, green, orange, red and infrared radiations are associated with impurity recombiA = nation. At T 15 K energy of excitons Eex B C 2.550 eV, Eex = 2.564 eV, Eex = 2.632 eV, bonding energies of excitons: EA = EC = 0.0294 eV, EB = 0.0295 eV. Centers of radiative recombination are centers of photosensitivity. Having the high photosensitivity in a wide spectral range: from UV to near IR, in the X-ray spectral range CdS is characterized by high sluggishness, low temperature and time stability of photocurrent. The absence of a center of inversion and a strong electron–phonon interaction determine the piezoelectric properties. The capability of fabrication by simple methods in the form of powders, tablets, and caked layers of thin lms with controllable properties is a pronounced advantage. The uniqueness and variety of its physical properties allows its use as a model material of the physics of semiconductors and quantum electronics: in photo-, opto-, acoustoelectronics, optics, laser engineering. Cadmium sulphide is widely used as a crystallophor for the creation of the screens of electron tubes, including color television, as a photoconductor for the creation of photoresistors, of nuclear particles radiation sensors, as an element of heterojunctions for solar phototransformers.

CALAMITICS

Uniaxial liquid crystals with structure units (molecules or micelles) of oblong cylindrical shape (cf. Discotics).

CALORIMETRIC COEFFICIENTS

CALCIUM, Ca

Chemical element of Group II of the periodic system with atomic number 20 and atomic mass 40.078, it belongs to alkaline-earth metals. Natural calcium is a mixture of 6 stable isotopes with mass numbers 40, 42–44, 46, 48; among them, 40 Ca (96.94%) is the commonest and 46 Ca (0.003%) is the rarest. Electronic conﬁguration of outer shell is 4s 2 . Atomic radius is 0.197 nm. Successive ionization energies are 6.133, 11.872, 50.914 eV. It is chemically active; oxidation state +2. Electronegativity is 1.04. In free form, calcium is a silvery-white metal; it darkens in the air due to formation of products of calcium interaction with oxygen, nitrogen, water vapors, etc., at the surface. From room temperature to 716 K, α-Ca is stable with face-centered cubic lattice (with parameter a = 0.556 nm); at temperatures above 716 K and up to T melting = 1120 K β-Ca is stable with a body-centered cubic lattice (with parameter a = 0.448 nm), T boiling = 1770 K. Density of α-Ca is 1.55 g/cm3 . Heat of melting is 8.4 kJ/mole; heat of evaporation is 152 kJ/mole; speciﬁc heat cp = 25.9 J·mole−1 ·K−1 . Work function 2.75 eV. Debye temperature is 220 K; temperature coefﬁcient of linear expansion is 2.2·10−5 K−1 (at 273 to 573 K); heat conductivity is 125 W·m−1 ·K−1 ; electrical resistivity is 3.8·10−2 μ·m (at 273 to 373 K); temperature coefﬁcient of electrical resistance is 4.57·10−3 K−1 . Hall constant is −1.78·10−10 m3 /C; magnetic susceptibility is χ = +1·10−9 . Modulus of normal rigidity is 21 to 28 GPa, tensile strength is 59 GPa, elastic limit is 4 MPa, limiting yield stress is 37 MPa. Brinell hardness is ∼250 MPa. Metallic calcium is used in metallurgy for reduction of U, Th, Zr and other rare metals from their compounds; as deoxidizing and degassing agent in melting of special steels, bronze, etc. Calcium is used as a getter in electronic devices. Monocrystals of the calcium compound, ﬂuorite CaF2 , ﬁnd wide use in optical and laser devices. CALIFORNIUM, Cf

Chemical element of Group III of the periodic system with atomic number 98 and atomic mass 251.08, belongs to actinides. There are no stable isotopes, and 17 radioactive isotopes are known

147

with mass numbers 240 to 256. Electronic conﬁguration of outer shells of atom is 5f 9 6d 1 7s 2 . Atomic radius is 0.169 nm; ionic radius of Cf3+ is 0.906 nm. Oxidation state is +3 (less often, +2, +4, +5, +6). Electronegativity is 1.23. In free form, californium is a silvery metal. It exists in two allotropic modiﬁcations: lowtemperature (α-Cf) and high-temperature (β-Cf). The ﬁrst has a hexagonal close-packed crystal 4 ), a = 0.3988 nm, (space group P 63 /mmc (D6h c = 0.6887 nm at room temperature); according to other data, it has a double hexagonal close-packed crystal lattice (a = 0.339 nm, c = 1.101 nm). The other modiﬁcation has a face-centered cubic lattice (space group F m3m (Oh5 ), a = 0.5743 nm and a = 0.494 nm upon hardening by quenching at ∼1000 K and 870 K, respectively) at temperatures above 860 K to T melting = 1170 K. T boiling ≈ 1500 K. Density of α-Cf is 15.1 g/cm3 . Below the Curie point T C = 51 K, α-Cf transforms from a paramagnetic state to a ferromagnetic one; in β-Cf, no magnetic ordering has been found. Californium isotopes (in particular, 252 Cf) are used as neutron sources in activation analysis, in medicine, etc. Californium is highly toxic. CALORIMETRIC COEFFICIENTS

The thermodynamic coefﬁcients of the form (∂Q/∂μ)ν where μ and ν take on the values of any of the thermodynamic parameters P , V , T (pressure, volume, temperature) of a system. The quantity ∂Q is the amount of heat transferring the system into a new thermodynamic state under a variation of μ by ∂μ at ν = const. There are 6 principal calorimetric coefﬁcients: (∂Q/∂T )V = CV , speci c heat at constant volume, (∂Q/∂T )P = CP , speciﬁc heat at constant pressure, (∂Q/∂P )T , heat of isothermal compression, (∂Q/∂P )V , heat of isochoric compression, (∂Q/∂V )P , heat of isobaric expansion, (∂Q/∂V )T , heat of isothermal expansion. The calorimetric coefﬁcients can be expressed via the derivatives of the thermodynamic state functions: enthalpy H and internal energy U (see

148

CALORIMETRY

Thermodynamic potentials):

∂Q ∂T V ∂Q ∂T P ∂Q ∂P T ∂Q ∂P V ∂Q ∂V P ∂Q ∂V T

∂U , ∂T V ∂H = , ∂T P ∂H = − V, ∂P T ∂U = , ∂P V ∂U = + P, ∂V P ∂U = + P. ∂V T =

In addition to calorimetric coefﬁcients, thermodynamics also makes use of six thermal coefﬁcients: (∂V /∂P )T , (∂P /∂T )V , (∂T /∂V )P , (∂V /∂P )S , (∂P /∂T )S and (∂T /∂V )S , where S is the entropy. There are 9 independent thermodynamic relationships between these 12 thermodynamic coefﬁcients so only 3 thermodynamic coefﬁcients can be selected as independent ones to be evaluated theoretically or determined experimentally. In principle all other coefﬁcients can be calculated via these three, chosen as independent. This circumstance allows one to calculate coefﬁcients that are difﬁcult to measure experimentally through easily measurable ones. For instance, ∂P ∂V 2 , CV = CP + T ∂V T ∂T P ∂V ∂P ∂T = −1, ∂P T ∂T V ∂V P ∂P ∂P ∂H =T +V . ∂V T ∂T V ∂V T

Instruments for calorimetric measurements are called calorimeters. Their design is determined by the temperature interval and desired accuracy. The two most widely used types in studies of solids are adiabatic calorimeters where the heat exchange between calorimeter and medium is negligibly small, and dynamic (heat-conducting) calorimeters based upon detection and control of the heat ﬂux between the sample and the environment. Adiabatic calorimeters with a pulse heat input are very accurate for measurements made close to equilibrium. They are used at temperatures from 0.05 to 1000 K to determine the speci c heat, thermodynamic functions, latent heats of phase transitions, the critical index α of phase transitions; density of states of electrons at the Fermi level N(EF ) by the electronic speciﬁc heat coefﬁcient γ ; obtaining direct information on energy levels of valence electrons by the Schottky effect; investigation of energy properties of vacancies and coordination polyhedra. A drawback of this method is the long time required for making the measurement. Dynamical calorimeters, in particular the Calve type, are used at temperatures from 77 to 1880 K. The temperature variation rate is from 1 K/h to 64 K/min. The important advantage of calorimeters of this type is the possibility of contact between the sample and the environment, control of the pressure or gas phase during the experiment, and access to the center of the calorimeter when necessary. The ﬁeld of application is the determination of heat capacities, thermodynamic functions, latent heats of phase transitions, heats of oxidation–reduction reactions, heats of gas–solid reactions, the energy related to the strain of a solid, and heats of adsorption and desorption. At temperatures above 1800 K the speciﬁc heat of solids is determined by the offset method. Benzoic acid and corundum have been adopted as standard substances in calorimetry.

CALORIMETRY (fr. Lat. calor , heat, and Gr. μετρεω , am measuring)

CANONICAL TRANSFORMATION METHOD (N.N. Bogolyubov, 1947)

Methods for measuring thermal effects accompanying different processes. Calorimetric methods are used in the interval 0.05–3500 K and attain an accuracy 0.01%. Calorimetry at temperatures above 400 K is conventionally called a hightemperature type.

A method utilizing a unitary transformation of particle creation ak+ and annihilation ak operators in order to reduce the initial complex Hamiltonian of a many-particle quantum system, involving interacting particles expressed in a second quantization representation, to a simpler Hamiltonian in

CAPACITANCE

diagonal form for noninteracting quasi-particles with a restructured energy spectrum. If the initial Hamiltonian has the form 1 1 ∗ , H= Ak ak+ ak + Bk ak a−k + Bk∗ ak∗ a−k 2 2 (1) then by introducing new operators according to the relations + , ak = λk ck + μ∗k c−k

+ + a−k = λ∗k c−k + μk ck (2) the Hamiltonian assumes the form H = ε(k)ck+ ck + E0 , (3) 1/2 ε(k) = A2k ∓ |Bk |2 .

The parameters of the canonical transformation obey the normalization condition |λk |2 ∓ |μk |2 = 1. In formulae for the energy of the quasi-particles and the transformation parameters the upper sign corresponds to bosons and the lower sign corresponds to fermions. The canonical transformation for spin waves was applied by Holstein and Primakoff (1940) to a ferromagnetic material, and it was applied by Bogolyubov (1947) to bosons for the case when many of them are in the state of a Bose–Einstein condensate (see Bose–Einstein condensation). The method was exploited by Bogolyubov to construct his microscopic theory of superconductivity (1947). It results in the following elementary excitations: 2 2 2 k 2 2 , (4a) E(k) = k u (k) + 2m NV (k) u(k) = , (4b) m where m is the boson mass, N is the number of particles in a unit volume, and V (k) is the Fourier transform of the pairwise interaction potential. For particles with repulsion, when V (k) > 0, Eq. (2) yields at k → 0 the acoustic dispersion law of quasi-particles E(k) ≈ ku(0), which is a necessary but insufﬁcient condition for the super uidity of neutral Bose systems (see Landau super uidity criterion). When attraction dominates at large distances with V (0) < 0, the spectrum (2) at k → 0

149

becomes unstable (imaginary), which corresponds to an exponential growth of long-wavelength perturbations in time, and a spontaneous contraction (collapse) of the system. For charged bosons (e.g., bipolarons) with a long-range Coulomb repulsion V (k) = 4πe2 /k 2 (e is the boson charge), the spectrum (2) of quasi-particles at k = 0 has a ﬁnite energy gap E(0) = ωp (ωp is the plasma frequency) and satisﬁes the superﬂuidity criterion, which corresponds to superconductivity (see Bipolaron mechanism of superconductivity). In the case of electrons (fermions) interacting under the conditions of Cooper pairing (see Bardeen–Cooper–Schrieffer theory) one can use Hamiltonian (1), where k denotes both the momentum and the spin of the electron, and Ak and Bk are given by Ak = ξ(k),

Bk = Δ(k).

Here ξ(k) is the energy measured from the Fermi level, and Δ(k) is the non-zero energy gap below the transition temperature from the normal to the superconducting (superﬂuid) state of a Fermi system. In the self-consistent eld approximation, which is asymptotically accurate in the thermodynmic limit (see Bogolyubov method in the theory of superconductivity), transformations (2) lead to a reconstructed spectrum of quasiparticles in a superconductor with the energy ε(k) = [ξ 2 (k) + Δ2 (k)]1/2 . CAPACITANCE

A quantitative measure of the ability of an object or material to retain electric charge q. Charged particles of the same sign attempt to go out of a charged body due to electrostatic repulsion. Mobile charge carriers in a conducting medium spread over its surface and provide an equal value of electric potential ϕ everywhere on the surface. If the conductor is electrically charged then its potential differs from that at inﬁnity where by convention ϕ∞ = 0. The value ϕ is proportional to q; and it speciﬁes the conductor capacitance by the ratio C = q/ϕ. The greater the value of C, the greater the charge on the conductor at a given ϕ. The magnitude C of an isolated conductor is determined by its geometric dimensions and shape; e.g., the capacitance of a sphere is equal to its

150

CAPACITANCE, BARRIER

radius (in Gaussian system of units). In a system of conductors, a correspondence between their charges and potentials is determined by the linear

relations qi = j Cij ϕj (Cij is called the capacity coefﬁcient of the ith and j th conductors). In a system metal–insulator–metal (condenser), the capacitance is determined by the relation C = q/ ϕ where q is the value of charges of opposite sign on every capacitor plate; ϕ is the potential difference between the plates. For a planar capacitor C = εA/d where A is the area of each plate, d is the distance between them, and ε is the relative (dimensionless) dielectric constant of the medium between the plates. For a very small d, the capacity of the system can be very large. The systems metal–semiconductor, semiconductor junction, and so on are similar to a capacitor, and can also have a signiﬁcant capacitance (see Barrier capacitance). Variations of the thickness of the dielectric layer under actions of any kind provide information on the distribution of electrically active extended defects in a system (see Capacitance–voltage characteristic, Capacitance spectroscopy). Josephson junctions, with typical capacitances C ∼ 10−15 F, exhibit voltage changes V = e/C ∼ 0.016 mV for individual electron tunneling. This is called a Coulomb blocade, and it appears on a current versus voltage characteristic curve (I versus V , or dI versus dV plot) as a sequence of steps called a Coulomb staircase. CAPACITANCE, BARRIER See Barrier capacitance. CAPACITANCE SPECTROSCOPY

A collection of methods for determining the energy spectrum of deep levels in semiconductors from changes in their barrier capacitance, C, during variation of the applied voltage. A simple version of capacitance spectroscopy is based on measuring steady-state capacitance–voltage characteristics. When a reverse bias (i.e. a bias in the cut-off direction) is applied to a system containing a semiconductor junction or a Schottky barrier, the thickness L of the semiconductor region with depleted current carriers increases, and the capacitance of the depletion layer decreases. More information can be obtained by methods of nonstatic capacitance spectroscopy of deep levels. It

is based on the measurement of the capacitance relaxation kinetics for different combinations of factors applied to ﬁll or ionize the deep levels (such as forward and reverse bias pulses of various durations, photoionizations, and temperatures). Using these methods provides separate measurements of concentrations of deep levels with different ionization energies, and also determines the cross-sections of charge carrier trapping at the levels. The efﬁcient Lang method measures the differences between C at two times, t1 and t2 , during the course of the relaxation of C with the emission of electrons or holes from individual levels into a corresponding allowed band. There are modiﬁcations of this method when the relaxation of current rather than capacitance is measured; and taken together they constitute the relaxation spectroscopy of deep levels. CAPACITANCE, SURFACE See Surface capacitance. CAPACITANCE–VOLTAGE CHARACTERISTIC

Dependence of the sample capacitance C on the applied voltage V . Measurement of the capacitance–voltage characteristic is one of the most widespread methods of investigating semiconductor electron–hole transit, heterojunctions, Schottky diodes and metal– insulator–semiconductor structures. From the shape of a C–V characteristic it is possible to determine the distribution of doping impurity in the structure. In particular, in sharp p–n junctions and Schottky diodes the capacitance–voltage characteristic plotted as C −2 versus V is a straight line with a slope characterizing the doping of the semiconductor, and the cutoff voltage is equal to the equilibrium height of the potential barrier at the junction (contact potential difference). The characteristic shape of the C–V characteristic for M–I–S structures is shown in the ﬁgure. The presence of deep levels within the bulk or at the surface of the sample, which recharge during voltage variations, causes additional features of the capacitance–voltage characteristic. Besides, the shape of the C–V characteristic has a strong dependence on the frequency f of the probing signal, because at high frequencies there is not enough time to recharge the deep levels, and to

CARBIDE TRANSFORMATIONS

Dependence of the capacitance on the voltage in an M–I–S structure at a low (solid line) and a high (dashed line) frequency, where C0 is the insulator capacitance.

form the inversion layer in the M–I–S structure. This allows one to use the C–V characteristic and its frequency dependence to obtain information about the concentration, energy spectrum and trapping proﬁles of the bulk and surface levels (see also Varicap, Capacitance spectroscopy). CAPILLARY PHENOMENA

Physical phenomena arising from surface tension. Capillary phenomena are most easily observed in thin tubes (R 10−3 m). The fundamentals of capillarity theory laid by P.S. Laplace (1806–1807) include two basic laws: (1) the excess pressure under the curved surface of liquid is 1 1 , (1) +

p = ±σ R1 R2 where σ is the surface tension coefﬁcient, R1 and R2 are the radii of curvature of two mutually perpendicular sections of the surface at the point in question; and (2) the edge angle θ0 of a solid surface by a liquid is independent of the shape of the surface. Of importance in the theory is the capillary constant a with the dimensions of length: σ , (2) a=

ρg where ρ is the difference between the densities of the phases in contact, and g = 9.8 m/s2 . For cylindrical tubes the Borelli–Jurin equation holds 2σ cos θ0 h= , (3) gRρ where h is the height of the rise of the wetting liquid and ρ is the liquid density. Eq. (3) describes the impregnation of pore structures, and

151

substantiates the role of capillary forces in the root feeding of plants utilized for soil tillage. Eq. (1) explains the presence of a considerable capillary counter-pressure in a system of alternating drops of liquid and gas bubbles in capillaries (gas embolism, decompression sickness in divers). See also Thermocapillary effect, Electrocapillary phenomena. CARBIDES (fr. Lat. carbo, coal, and Gr. ειδoς , type) Chemical compounds of carbon with metals

and some nonmetals. We can distinguish covalent carbides (beryllium carbide, boron carbide, silicon carbide), metal-like, and salt-like carbides. Metal-like carbides include those of scandium, yttrium, lanthanum, lanthanides, transition metals of Groups IV to VII of the periodic system, and metals of the iron family. Carbides of transition metals (TiC, Cr3 C6 , Cr3 C2 , Mo2 C, WC and others) are interstitial phases and structures close to interstitial, with the carbon atoms occupying octahedral or tetrahedral sites (voids) of close-packed metal lattices. Such carbides exhibit metallic characteristics of conductity, high melting (decomposition) temperature, hardness and chemical stability. Salt-like carbides include those of s-state metals (alkali, alkaline-earth metals and aluminum). The best known among them is calcium carbide CaC2 , a colorless crystal, with density 2.21 g/cm3 , T melting ∼ 2300 ◦ C. Carbides are obtained from elementary matertials in vacuo or in a reducing gas atmosphere, as well as by interaction of metallic oxides with carbon in vacuo or in a reducing atmosphere, by interaction of metals or their oxides with carbon-containing gases, and by interaction of gaseous compounds of some metals (halides) and carbon in the hydrogen atmosphere. The favorable properties of carbides are used in nuclear and space engineering, microelectronics, metal processing and many other areas. CARBIDE TRANSFORMATIONS in steel

Formation and rearrangement of iron carbides during the course of different treatments of steel. Carbides are one of the basic phases in steel; they may form upon cooling of steel heated above some critical point, or upon tempering of hardened steel (see Quenching). Above 300 ◦ C a stable iron carbide, cementite, is present in carbon steel. At the tempering of alloyed steels, the temper-

152

CARBON

ature of cementite (Fe3 C) formation increases. Redistribution of carbon and alloying elements between phases leads to alloying of iron carbide. With a certain temperature of tempering, degree of steel alloying, and ratio of carbide-forming element content to that of carbon, the formation of special carbide is possible. Destabilization of cementite (or special carbide) occurs at complete replacement of one atom of iron in cementite (or the basic element in special carbide) with the alloying element. In multicomponent alloying such replacement occurs with several alloying elements simultaneously. Carbide transformations that run according to the mechanism of alloy aging and direct precipitation of carbides from ferrite, bypassing cementite, are used to harden structural, stamp, tool, high-speed and certain austenite steels, as well as to maintain hardening in long-term operation of boiler and turbine, motor equipment, of industrial holders and fastening parts, etc., at increased temperatures. The speciﬁcs of redistribution of carbon and alloying elements between phases in multicomponent alloying causes the carbide transformations to run at a lower number of alloying elements than in single or simple alloying (and the same total degree of alloying). Here, the ferrite contains more alloying elements, which permits a more complete use of their effect upon physical mechanical, technological and service properties of steel. The composition and type of the carbide crystal lattice, distribution of carbides within the structure, and the mechanism of their formation are investigated using chemical phase analysis, X-ray structure analysis, microscopic diffraction and magnetic analyses, Mössbauer spectroscopy, internal friction, and electron microscopy with the help of replicas and foils. CARBON, C

The chemical element of Group IV of the periodic table with atomic number 6 and atomic weight 12.011. The mass numbers of the two stable carbon isotopes are 12 (12 C, 98.892%) and 13 (13 C, 1.108%). The 14 C isotope is unstable (halflife 5730 years). The wide diversity of properties of carbon compounds is due to the electronic conﬁguration of the carbon atom: 1s 2 2s 2 2p2 . Interaction with other atoms results in rearrangement

of the density of the electron clouds and the concentration of electron density in certain directions, such as along chemical bonds (see Hybridization of orbitals). Depending on the way atomic orbitals are combined, sp-, sp2 - and sp3 -hybridizations are distinguished. Each hybridization corresponds to a particular spatial arrangement of a bond. Oxidation states of carbon in its compounds are −4, −2, +2, and +4; electronegativity value is ≈2.58; atomic radius 0.077 nm, ionic radii: 0.016 nm for C4+ and 0.26 nm for C4− . There exist ﬁve allotropic (see Allotropy) modiﬁcations of solid carbon: diamond (sp3 -hybridization of orbitals), graphite (sp2 -hybridization), fullerene (C60 and analogues, sp2 -hybridization), carbyne (sp-hybridization), and amorphous carbon (mixed type of bonding). Carbyne is a quasione-dimensional semiconductor, the width of the band gap of which is ∼1 eV. Amorphous carbon is a polyphase structure, which consists of the ﬁnest inclusions of polymorphic modiﬁcations of carbon. Depending on the mode of preparation, carbon may also contain chemically bound hydrogen atoms, which saturate the dangling bonds of the carbon structure. The principal carbon-containing minerals are salts (carbonates) of carbonic acid H2 CO3 . Carbon atoms are the chief constituents of coal, oil, peat and other materials. Carbon is a nonmetal and behaves as an active reducing agent on heating. It forms carbides with various elements, e.g., boron carbide, silicon carbide SiC, cementite Fe3 C. Carbon is used as a reducing agent, as a component of various alloys, as fuel, for production of electrodes, etc. CARBON, ACTIVE See Active carbons. CARBON FILM, DIAMOND-LIKE See Diamond-like carbon lms. CARBYNE (fr. Lat. carbon , coal)

The third allotropic modiﬁcation of carbon, which consists of rectilinear carbon chains bound into crystals through van der Waals forces. The rectilinear shape of the chains is due to sp-hybrid bonding of the carbon atoms. In actual samples the individual chains are cross-linked, with perhaps some periodicity, and this involves a transition of

CASTING MATERIALS

some carbon atoms into sp2 - or sp3 -hybrid type bonding. The presence of carbyne can be detected by the methods of electron diffraction and X-ray diffraction. Crystalline particles of carbyne are colorless, and no large monocrystals have been prepared. Carbyne is hard to obtain in a pure form (free from admixture of laminated modiﬁcations of carbon). Density and other physical properties depend on the method of manufacture and puriﬁcation. Carbyne has a higher speci c heat than graphite and diamond, and it surpasses graphite in hardness. Heat of combustion is 84 to 372 kJ/mole, which is signiﬁcantly lower than that of graphite and diamond, which attests to the thermodynamic stability of carbyne. There are 3 bands in the Raman spectrum of carbyne at 1360, 1580 and 2140 cm−1 , the last of them being the characteristic one related to the vibrations of conjugate C–C bonds. Carbyne is an n-type semiconductor with a band gap of 0.64 eV; electrical resistivity is 106 ·cm (at 293 K). Carbyne was originally obtained and characterized by the methods of oxidative polycondensation of acetylene. It forms upon condensation from vaporgas phase, plasma, an ion-molecular beam under the conditions that are softer compared to those for forming diamond, and of laminated polymers of carbon. Natural carbyne was discovered in 1968 in a meteorite crater and received the name chaoite (white veins and disseminations in graphite). In its chemical inertness it surpasses graphite and approaches diamond. Defect-free thread-like crystals of carbyne are believed to have very high rupture strength. CASCADE, COLLISION See Collision cascade. CASTING

The process of forming pieces (casts) by ﬁlling a hollow casting form or mold with melted material (metals, their alloys, plastics, certain rocks, metallurgy slags). The principal advantages of casting include the possibility of obtaining casts of a complicated conﬁguration that is as close in size and shape to the ﬁnal product as possible. Mold casting of steel, cast iron, nonferrous alloys (from 5–10 to 100 g and more in mass) is used

153

to produce various parts, from time-piece components to heavy-duty constructions for engineering, metallurgy, power and other branches of machine building. Steels and alloys are cast into molds (plate casts, forging casts) or poured continuously into water-cooled crystallizers (for a continuously operating casting installation). More than 50 types of casting techniques are available. Traditional technologies include pouring molten metal from dippers or crucibles driven by gravity into sand casting forms. Special casting techniques make it possible to improve the quality of casts, perform precision casting in both size and shape, and achieve special physical and mechanical characteristics. Such technologies involve various external factors which act upon the crystallizing metal and provide for using special casting forms, models or casting techniques. Among the latter are casting under high or low pressure, centrifugal casting, electric slag casting, continuous or suspension casting, casting into melted-out models, casting into chill molds, ceramic and shell forms, etc. Art casting is done using melted-out models to produce monumental sculptures, architectural decorations, and jewelry. CASTING MATERIALS

Macroscopically inhomogeneous substances obtained by fusion of two and more mutually soluble metals, nonmetals, or organic substances, and by subsequent solidi ca tion of the liquid phase in a mold of a particular shape. Depending on the temperature range of metastability of the liquid phase, the structure of casting materials may be crystalline or amorphous. In a general case, the conditions of solidiﬁcation in the amorphous or crystalline states may be controlled by the cooling rate, by the purity of the materials, by their solubility, and by their crystallization activity. The properties of casting materials crystallizing during the course of solidiﬁcation are not only determined by their chemical composition, by the method of fusion, thermal and other types of deformationless treatment, but are also dependent on the thermal conditions of solidiﬁcation, on the nucleation rates of centers, and the linear growth rates of crystallization nuclei. These factors determine the degree of development of physical, chemical and structural inhomogeneities in

154

CAST IRON

casting materials. The processes of their solidiﬁcation and crystallization, and hence their properties, may be signiﬁcantly changed by modi cation, electromagnetic mixing and other methods (see Casting). CAST IRON

Alloy of iron with carbon (usually 2 to 4% C), also containing (Si, P and S, Mn), and sometimes additional alloying elements (Al, V, Cr, Ni, etc.); it solidiﬁes with the formation of eutectics. Unlike steel due to its low plasticity, cast iron is machinable under pressure. It is characterized by a high liquid yield. Cast irons are subdivided into the following classes: pearlite, ferrite, perlite-ferrite, sorbite, troostite, bainite, martensite, troostite-ferrite, and austenite. According to its microstructure the following types are distinguished: gray cast iron (in the form of cementite or iron carbide Fe3 C), and forgeable cast iron obtained by annealing white cast iron (ﬂocculent graphite). The properties of cast iron are improved by alloying, modi cation, thermal treatment. Cast iron is the primary product obtained from the processing of iron ore materials. It is used in chemical, petroleum, and agricultural machine building, in tool, car and tractor fabrication, in civil engineering, etc. CATALYSIS, RADIATION See Radiation catalysis. CATASTROPHE, POLARIZATION See Polarization catastrophe. CATEGORY (fr. Gr. κατ ηγ oρια , accusation)

A level of crystallographic classiﬁcation by the number and order of special (or individual) directions, i.e. directions in the crystal lattice which do not repeat under a symmetry operation (see Crystal symmetry). There are three categories: the highest one (no special direction and some symmetry axes of order higher than 2); the medium type (one special direction along a unique symmetry axis of order 3, 4, or 6); the lowest one (no special direction and no symmetry axes of order higher than 2). The highest category involves crystals of the cubic system, the medium one includes those of the hexagonal system, trigonal system and tetragonal system, and the lowest category encompasses structures of the orthorhombic system,

monoclinic system and triclinic system. Depending on the category the nature of the anisotropy, and many physical properties of a solid change characteristically (see Anisotropy of crystals). This classiﬁcation term “category” is not commonly used in the Western literature. CATHODE See Cold cathode, Field-emission cathode, Thermionic cathode, Photocathode. CATHODE SPUTTERING See Sputtering. CATHODOLUMINESCENCE A type of radioluminescence excited by an

electron beam (“cathode rays”). Depending on the electron energy E, one distinguishes low-voltage (E = 10–100 eV) and high-voltage (E > 0.5 keV) cathodoluminescence. At high-voltage the electrons overcome the surface barrier, penetrate to a depth proportional to E 1.4 , knock out secondary electrons that also ionize atoms, create electron– hole pairs, or directly excite the ions of the activator (Mn2+ , Tb3+ and others). The minority carriers migrate across the lattice and are trapped at luminescent centers, accompanied by radiative recombination. At low voltage the excitation by primary electrons only covers several near-surface atomic layers, and the diffusion of nonequilibrium carriers produces a zone of ﬂuorescence spreading into the depth of the sample. The forming negative charge is neutralized at high voltage luminescence mainly through the emission of electrons from the surface of a luminophor, while at low voltage the neutralization is due to the conductivity of the latter. In its spectrum, cathodoluminescence is similar to other types of luminescence. Its brightness in a certain spectral region is proportional to E and the current density in the beam. The energy yield is 10–30% for high voltage and 0.5–2% for low voltage. Cathodoluminescence is employed in picture tube screens and in low-voltage indicators that are used in devices for the visualization of information, TV sets and other electronic devices. Cathodoluminescence underlies the operation of lasers excited by an electron beam.

CATLOW–DILLER–NORGETT POTENTIAL

155

CATLOW–DILLER–NORGETT POTENTIAL (C.R. Catlow, K.M. Diller, M.J. Norgett, 1977)

A central pair-potential that describes shortrange ion-to-ion interactions in ionic crystals using the shell model. An analysis of the relation between the equilibrium interionic distance in a crystal and its elastic constants on the one hand, and the interionic interaction potentials yielded by this model for alkali-halide crystals (such as LiCl, NaCl, KCl, RbCl) on the other hand, demonstrated that the ion-to-ion interaction is attractive at long distances r and repulsive at short distances. Starting with that observation, Catlow, Diller and Norgett offered the following two proposals for the short-range potential of (identical) second nearest neighbors in alkali halides. I. The Buckingham potential V (r) = A exp(−r/ρ) − Cr −6 contains an exponential repulsive term with parameters A, ρ determined using an electron gas model, and an attractive van der Waals potential with a parameter C (see Van der Waals forces). For example, the F− –F− ionic interaction in a LiF crystal is described by A = 1128 eV, ρ = 0.02753 nm, and C = 12.71 eV·nm5 . The parameters for the anion–anion (C−− ) and cation–cation (C++ ) interactions are arbitrarily assumed to be equal to each other, C−− = C++ = C/2. II. A combined (“spline”) potential consists of expressions used in proposal I for attraction at long distances and repulsion at short ones, plus the third and ﬁfth power polynomials for intermediate distances (see Fig.): V (r) = −Cr −6 , V (r) =

3

r > ra ,

(1)

ai r i ,

ra > r > rm ,

(2)

bi r i ,

rm > r > rb ,

(3)

i=0

V (r) =

5 i=0

r , V (r) = A exp − ρ

rb > r.

(4)

Matching the functions at points ra , rb , and at the minimum point rm is carried out by invoking continuity of the functions and their

Schematic represention of the potential described in proposal II for the four regions: (1) r > ra , (2) ra > r > rm , (3) rm > r > rb , and (4) rb > r.

ﬁrst derivatives. The parameters A and ρ coincide, while C considerably exceeds the value expected from proposal I. For example, C = 26.8 eV, while ra = 0.3457 nm, rb = 0.2 nm, rm = 0.2833 nm for the F− –F− interaction. These parameters are self-consistently adjusted over the entire alkali halide series. Having ﬁxed the potential parameters for second nearest neighbors, one may update the respective parameters for ﬁrst neighbors, that is for adjacent ions, that potential being the common Born– Mayer potential, V (r) = A exp(−r/ρ). Next the parameters of the ions are determined using the shell model. The shell charge and the nucleus– shell bonding constant are found by comparing the static and the high frequency dielectric constants and the transverse optical frequencies with experimental data for all the crystals, so that the polarization of a crystal may be adequately described by the result. The Catlow–Diller–Norgett potential, as presented in II above, has a number of advantages over other potentials used for ionic crystals. It covers every individual ion and is easily applied to modeling alkali halides. It offers a consistent picture of the ion-to-ion interaction for all the alkali halides. In combination with the Coulomb potential it adequately describes the properties not only of an ideal crystal, but of a real one as well. In the

156

CAUCHY RELATIONS

latter the ion-to-ion distances may differ considerably from the equilibrium ones in the vicinity of defects. Thus it becomes possible to study both intrinsic crystalline and impurity defects in various ionic crystals (see Interatomic interaction potentials). CAUCHY RELATIONS (A. Cauchy)

Additional relations between the 36 crystal elastic moduli cik following from the symme-

tries of interatomic interactions, where i, k = 1, 2, . . . , 6. If the interatomic forces are pairwise and central then each term is at a center of symmetry, the undeformed crystal is stress free, and the harmonic approximation is valid. Then in the general case there are 21 independent modulus constants cik (in Voigt notation) by virtue of the symmetry condition cik = cki . The six Cauchy relations c12 = c66 , c13 = c55 , c23 = c44 , c14 = c56 , c25 = c46 , and c36 = c45 reduce the number of independent elastic moduli to 15. For cubic crystals there are three independent elastic constants (c11 , c12 , c44 ), and one Cauchy relation (c12 = c44 ). These results hold well for some alkali-halide crystals, but not for most other cubic crystals. In metallic crystals the Cauchy relations usually do not hold (e.g., in noble metals c12 /c44 ∼ 2–4). In elastically isotropic crystals obeying the Cauchy relations c11 = 3c44 , and the Poisson ratio is ν = 1/4. For orthorhombic crystals there are 9 independent constants and 3 Cauchy relations, corresponding to 6 independent moduli when the Cauchy relations hold. CAVITATION RESISTANCE

The ability of a material to resist the effect of cavitation (formation of vapor bubbles) that appears in a liquid at the passage of a powerful sonic or ultrasonic wave (acoustic cavitation), and also during high-speed ﬂow past bodies (hydrodynamic cavitation). The collapse of a cavitation bubble at the compression phase produces a local hydraulic shock which affects the surface of a tool, an article, or a part. Cavitation erosion is especially strong for brittle materials such as rocks, concrete, and ceramics. Metals possess considerably higher cavitation resistance that reduces noticeably in hostile media and suspensions with abrasive particles, and upon increasing the pressure within the

volume of a liquid. Ultrasound is widely applied in some technological processes where cavitation plays an important role, and this has prompted the search for materials with high cavitation resistance. Its measure is the loss of mass per unit area during a preset period of time. The cavitation intensity is evaluated by the destruction of a thin aluminum foil placed in the cavitation area. There are also other methods to determine cavitation resistance in investigations of hydrodynamic cavitation, such as rotational, jet-impact, and ﬂowthrough ones. CAYLEY TREE (A. Cayley, 1889); also called a Bethe lattice

A branched structure in which each site has f nearest neighbors, and no two branches are permitted to cross each other. It is cycle-free, and also self similar since each branch is itself an entire tree. Such graphs are used for percolation studies, in cluster techniques to provide a convenient boundary condition for a cluster, to calculate the number of isomers of saturated hydrocarbons, and to describe disordered solids. CELLULAR STRUCTURE

Regions 1 μm in size which are free of dislocations, or which contain individual dislocations, dislocation dipoles, multipoles, interlacements, networks, etc., and are separated by dislocation interlacements, balls, or rods. The cell boundaries can be either dense or spread out, either narrow or wide, and so on. The cells can be equiaxial or nonequiaxial. Sometimes the cellular structure is called block-cellular structure (see Block structure). CEMENTATION

Coating a metal, usually iron or steel, by heating it with another substance so that the added material, usually a powder, diffuses into the surface; it is a type of chemical heat treatment. The coating material might be a metal like aluminum or zinc, or perhaps carbon. Diffusion saturation of a steel product surface by carbon typically produces a saturated layer that is 0.5 to 2 mm thick, with a carbon content of 0.8–1.1%. Cementation with subsequent quenching and low annealing provides articles with a high surface hardness, wear resistance and increased fatigue strength, leaving their

CENTRAL FORCES

core tough. Cementation may be carried out in gaseous, liquid, and solid media containing carbon. It is used in the production of tools. CEMENTITE (fr. Lat. caementum , broken stone) A structural component of steel and cast iron containing the elements iron and carbon. Cemen-

tite is the most stable iron carbide (Fe3 C), containing 6.7 wt.% C (see Carbide transformations). It is formed upon the cooling of iron–carbon alloys (see Iron alloys) if the conditions are favorable for crystallization to occur in the metastable phase diagram of these alloys (iron–cementite). Cementite is often a component of pearlite, sorbite, troostite and ledeburite. The crystal lattice of cementite is orthorhombic; the unit cell contains 12 atoms of Fe and 4 atoms of C. Lattice constants are: a = 0.4514 nm, b = 0.5079 nm, c = 0.6730 nm. According to some indications cementite is close to an interstitial phase (see Interstitial alloys). It forms substitutional solid solutions: carbon may be replaced by nitrogen or oxygen, iron by manganese, chromium or tungsten (alloyed cementite). Their dispersity, the form of cementite crystals, and their crystal structure associated with a ferrite environment (see Ferrites), to a large extent determine the strength and plasticity of iron–carbon alloys after a heat treatment. Cementite is hard and brittle, and there is practically no elongation if it fails during the course of tensile tests. The melting temperature is ∼1873 K; at this high temperature it decomposes into austenite and graphite. It is ferromagnetic with the Curie point of 486 K. CENTER See Active centers, Amphoteric center, Color center, Dilatation center, Luminescent centers, Paramagnetic center, Positron center, Positronium center. CENTER OF INVERSION See Center of symmetry. CENTER OF MASS, center of inertia

A point in a solid body relative to which the total ﬁrst moment of the all the components of the mass vanish, i.e. i mi r i = 0, where r i is the radius-vector of the ith mass relative to the center of mass. In the absence of torques a solid body

157

moves as if the resultant sum of all applied forces R = i F i were acting at the center

of mass, and the total mass of the body M = i mi were concentrated there. This deﬁnition implies that the center of mass is, in a uniform gravitational ﬁeld, the center of gravity, as well as the point where the resultant force of gravity Mg is acting. CENTER OF PERCUSSION

The point of a body about which it starts to rotate when an impulse (impulsive force) is applied at another point in the body. CENTER OF SYMMETRY, center of inversion

A special point of a ﬁgure possessing the property that during the inversion operation (r → −r) through that point as origin of coordinates, all the elements (points) of the ﬁgure transform into themselves (r is the coordinate of an arbitrary point of the ﬁgure). The presence of a center of symmetry is equivalent to the presence of an inversion axis of the ﬁrst order. Many properties of the solid state depend on the presence or absence of a center of symmetry; see, e.g., Electric e ld effects in radio-frequency spectroscopy. CENTI. . . (fr. Lat. centum , a hundred)

Preﬁx to the name of a physical value to form a fractional unit equal to 1/100 of the source unit. Abbreviation symbol is c. For instance, 1 cm (centimeter) = 0.01 m. CENTRAL FORCES

In solids these are forces of interaction between pairs of atoms (ions) acting along the straight line connecting them. In such a case these atoms are considered to be point masses. Formally the concept “central forces” is based on “rigid” point atoms (ions). When interatomic interactions in solids are described exclusively by means of central forces, this constitutes a coarse and phenomenological approximation. The central force is a special case of a pairwise interaction between atoms, when its adiabatic potential U has the form 1 U= ϕ |R i − R j | , 2 ij

where R i is the radius-vector of the lth atom, and ϕ is a function which depends on the type of interaction. For a gravitational ﬁeld involving two

158

CENTRAL PEAK

masses ϕ = −Gm1 m2 /|R 1 − R 2 |, corresponding to an inverse square central force law, where G is the gravitational constant.

dering point. This central peak is due to the contribution of nonlinear spin excitations, i.e. magnetic solitons.

CENTRAL PEAK

CERAMIC FERROELECTRIC See Ferroelectric ceramics.

A sharp increase of the magnitude of the order parameter u ctuation at a frequency approaching zero in the neighborhood of the critical point Tc of a structural phase transition. Initially a central peak was observed in 1971 in the energy spectrum of a beam of monochromatic neutrons scattered by a SrTiO2 crystal in the vicinity of Tc = 105 K. Central peaks have also been observed experimentally in spectra of Raman scattering of light. Depending on the nature and mechanism of its formation one should distinguish three types of central peaks: static intrinsic, static dynamic, and impurity types. A static intrinsic central peak is associated with the relaxation of lattice distortions of crystals without impurities. The mechanisms of dynamic intrinsic central peak formation are much more diverse. These involve ﬂuctuations of the entropy (ferroelectrics: SrTiO2 , KTaO3 , KDP type), the presence of an overdamped soft mode at T → Tc (K2 SeO4 ), two-phonon anharmonic interactions (germanate of Pb, SrTiO2 ), diffusion of mobile ions in solid electrolytes (Ag, F, β-alumina), formation of a paraphase, and relaxation at T → Tc of clusters of the prior ordered phase. The impurity central peak is associated with the relaxation of defects which differ from the point of view of a given central peak formation by the symmetry of their local surroundings, and by the rigidity of their coupling with a crystal lattice. Direct experiments on KPD-type crystals have shown that the central peak disappears at the annealing of defects. In the phenomenological theory the integrated intensity of a dynamic intrinsic central peak at T → Tc increases as the susceptibility (at a given external ﬁeld), and its width is 1 to 2 orders less than an impurity central peak width. For example, in NaNO3 the central peak width is ∼1013 s−1 , which is an order of magnitude less than the central peak width in KH2 PO4 . A central peak was found when quasi-one-dimensional magnetic materials (ferromagnetic CrNiF3 , antiferromagnetic KMnF3 , etc.) were examined at temperatures higher than the three-dimensional or-

CERAMIC GLASS See Glass ceramics. CERAMIC PIEZOELECTRIC See Piezoelectric ceramics. CERAMICS (fr. Gr. κεραμικoς , made of clay)

A baked (sintered) material; pottery. A class of compact materials, based on the compounds that the nonmetallic elements of Groups III and IV of the periodic system form with one another and/or with metals, produced by technological processes that allow for mass transport, as well as for the binding of the components. Classiﬁed as ceramic materials are: glass (see Vitreous state of matter), monocrystals of refractory materials, and composites with a ceramic matrix (see Composite materials). Traditional (Table 1) and novel ceramics may be distinguished. The vast majority of ceramic materials are mono- or heterophase polycrystalline materials based on high-melting compounds. A wide diversity and intricacy of the electronic structure of high-melting compounds comprising different types of interatomic bonds (covalent, ionic, metallic) results in a unique combination of properties (high energy of fragmentization, hardness, refractory properties, large elastic moduli, a collection of distinctive electrophysical properties, etc.). Their spatial distribution of interatomic bonds is related Table 1. Types of traditional ceramics • Pieces of Art • Household pottery and china (tableware and tiling, crockery, bathroom particulars, etc.) • Glass (a variety of items and materials for all areas of application) • Binding materials (cement, gypsum, lime, mortar, etc.) • Construction materials (pipes, bricks, roof tiles, etc.) • Fire prooﬁng materials (bricks, crucibles, etc.) • Abrasive materials

CERAMICS

159

Fig. 1. Typical scheme of the production technology of ceramics.

to diamond-like crystals with predominantly covalent bonds (carbides, silicon nitride and boron nitride), and these substances all have similar structures constructed on the principle of diversiﬁed sequential packing of identical layers. These compounds are characterized by the existence of a substantial number of polytypes (see Polytypism); the latter have also been found in diamond. Besides covalent and ionic crystals, there are many ceramic material components from a large group of metal-like high-melting compounds, such as interstitial solutions that form easily in transition metals by light elements with relatively small atomic radii. Most of these phases are compounds of variable proportion having wide ranges of homogeneity, and a great variety of structure types (e.g., CaFe, ZnS, CaB6 , etc.). Conventionally the properties of a ceramic are deﬁned not only by the properties of its

components, but to a substantial degree, by the technology of production (Fig. 1). Also widely employed are the methods of self-propagating high-temperature synthesis, chemical sedimentation, inﬁltration from the gas phase, etc. The stability of the crystal lattice and the low mobility of defects in high-melting compounds results in low rates of the diffusive and viscous processes responsible for mass transport, and for settling at the solid-phase sintering. For that reason, additives to activate the sintering are introduced into the batch charge, and this is then subjected to explosion processing to augment the number of defects, or there could be a physical and chemical modi cation of the surface, etc. The activating additives, usually oxides, secure the liquid-phase sintering regime, which not only facilitates the rearrangement of component particles, but also results in their recrystallization via the liquid phase. This ac-

160

CERAMICS Table 2. Properties of several types of alumina Type of ceramic

Fig. 2. Microstructure of ceramics fabricated by way of the processes: (1) solid-phase sintering, (2) liquid-phase sintering with the formation of (A) solid solutions, and (B) systems comprising a crystalline matrix with glassy phases at grain boundaries; (3) crystallization of eutectic liquids; obtaining composites of crystalline matrix with thread-like crystals (4), or with ﬁbers (5), by solid- or liquid-phase sintering, or by the chemical sedimentation and inﬁltration from the gas phase.

Strength, GPa

Type of defects

An ideal crystal, theoretical strength

50

–

Whisker thread-like crystals

15

Screw dislocations along the axis of growth, and surface defects

Single crystals

7

Surface and bulk defects of crystal lattice

Hot-pressed ceramic

0.8–1.0 Same as above, plus grain boundaries and additional phases

Sintered technical ceramic

0.2–0.3 Same as above, plus pores

celerates the sintering process, while permitting a substantial decrease in the temperature, but the ceramic thus fabricated will be interlayered with an amorphous phase at grain boundaries. Typical microstructures obtained with such processes are presented in Fig. 2. The type of microstructure that is realized, as well as the character of the defects and inhomogeneities in the ceramic, determine its mechanical behavior and its complex of physicochemical properties resulting, for instance, in a variation in strength by over two orders of magnitude (see Table 2). The wide variety of types of structure, and sometimes the attainment of record values of the physical properties of the phase components of the ceramics, provides us with the opportunity for fabricating unique materials for a large number of purposes. Along with the attainment of high strength (more than 1500 MPa), a high fracture toughness can be achieved to compensate for the traditional brittleness. The “viscous” state is not only reached by means of a “skeletal” reinforcement, but also because the processes of elastic energy dissipation are being purposely initiated at the vertex of a spreading crack; the effects of such processes are similar to the action of plastic relaxation at crack vertices in metals. In ceramics, the energy dissipation is conditioned by the development of microcracks, by ﬁrst- and second-order phase transitions, etc. The stability to cracking of such

CERIUM Table 3. Fields of application of novel (reﬁned, advanced) ceramics • In electrical engineering and circuit electronics (substrates, varistors, magnetic, ferroelectric and hightemperature superconducting ceramics, transducers, sensors, etc.) • Structural ceramics (engine parts in the aerospace and automobile industries, facing materials, fairings, thermoresistive bearings, heat exchangers, special ﬁreproof materials, etc.) • In medicine (implants, bio-ceramics, etc.) • In nuclear technology (nuclear fuel, materials for nuclear reactors, etc.) • Wear resistant ceramics • Low weight armor • Fiber and laser optics, etc.

a ceramic may be enhanced from a typical level of K 1c = 1–3 MPa·m1/2 up to values in the range of 10–30 MPa·m1/2 , viz., up to a magnitude characteristic of hard alloys and some metallic construction materials. The discovery in 1986 of high-temperature superconductivity in copper oxides, and the raising of the critical temperature of superconductors up to 90–135 K for ceramics of the type of YBa2 Cu3 O7−δ (123 phase) and HgBa2 Ca2 Cu3 O8+δ , respectively, opened up essentially new opportunities in superconductor electronics. All the superconducting cuprate ceramics are type II superconductors, possess a perovskite-like structure (see Perovskites), and have a carrier current density smaller than that of metals and alloys, the carriers generally being holes (in some cases electrons). The 123 phase, the ﬁrst one discovered with T c above 77 K, has granular particles of 1–10 μm dimensions that are in weak electrical contact with each other in the ceramic body, with the electromagnetic properties of the ceramic strongly inﬂuenced by intercrystallite grain-boundary layers. On the whole, there is a broad range of applications of these novel ceramics (Table 3), and these materials are used in many ﬁelds of technology. CERIUM, Ce

Chemical element of Group III of the periodic system with atomic number 58 and atomic mass 140.12; it is the lightest rare-earth element

161

aside from lanthanum. Natural cerium has 4 stable isotopes 136 Ce (0.193%), 138 Ce (0.25%), 140 Ce (88.48%) and 142 Ce (11.07%). The outer shell electronic conﬁguration is 4f 2 5d 0 6s 2 . Ionization energies are 6.9, 12.3, 19.5, 36.7 eV. Atomic radius is 0.181 nm; radius of Ce3+ ion is 0.107 nm, of Ce4+ ion is 0.094 nm. Oxidation states are +3, +4. Electronegativity is 1.08. Cerium is a silvery-blue metal; in air it is covered by a grayish-white oxide ﬁlm. Four crystalline modiﬁcations of cerium are known (α-Ce, β-Ce, γ -Ce, δ-Ce). The crystal lattice of α-Ce is face-centered cubic with a = 0.485 nm (at 77 K); β-Ce has a double hexagonal close-packed lattice (α-lanthanum type), a = 0.3673, c = 1.1802 nm (at 298 K); γ -Ce is face centered cubic with a = 0.51612 nm (at 293 K); δ-Ce has a body centered cubic lattice, a = 0.411 nm (at 1041 K). At room temperature γ -Ce is stable. During the course of cooling, starting from the temperature 263 K, γ -Ce partially transforms to β-Ce; the transformation is of a martensitic nature. At the temperature ∼95 K the non-transformed part of γ -Ce transforms to α-Ce. Below 77 K β-Ce also transforms to α-Ce, but this transition is not completed even at the temperature of liquid helium 4.35 K. The complete transition may be achieved only by plastic deformation of the sample at 77 K. The transitions γ ↔ α and γ ↔ β are characterized by large hysteresis depending on the temperature and pressure. At atmospheric pressure the reverse transformations α → γ and β → γ start from the respective temperatures ∼160 K and ∼373 K. If the pressure is over 2500 atm β-Ce cannot exist at any temperature. The behavior of Ce strongly depends on its history and purity. The transformation γ ↔ δ takes place at 998 K. Density is 6.678 g/cm3 at 293 K, Tmelting = 1071 K, Tboiling = 3740 K. Heat of melting is 9.211 kJ/mole, heat of evaporation is 390.18 kJ/mole, heat of sublimation is 398 kJ/mole; speciﬁc heat is 27.9 J·mole−1 ·K−1 at 298 K; coefﬁcient of thermal conductivity is 10.89 W·m−1 ·K−1 at 300 K, linear expansion coefﬁcient is 8.5·10−6 K−1 at 298 K. Electrical resistivity is 0.753 μ·m at 298 K, temperature coefﬁcient of electrical resistance is 8.7·10−4 at 273 K. Above 12.5 K cerium is paramagnetic with molar magnetic susceptibility +2300·10−6 .

162

CERMET

Thermal neutron cross-section is 0.63 barn. Debye temperature is 139 K. At room temperature the elastic modulus is 29.99 GPa, shear modulus is 11.99 GPa, Poisson ratio is 0.248; ultimate tensile strength of cast sample is 0.1206 GPa, relative elongation is 32.6%. Pure cerium is a forgeable and tough metal. At room temperature without preheating it is possible to manufacture cerium sheets by forging, and wire by pressing. It is used as an alloying addition to the light metals, and also as a getter. CERMET (fr. ceramic metal)

A composite material consisting of ceramic grains dispersed in a metallic matrix. It is formed by techniques of powder metallurgy. CESIUM, Cs

Chemical element of Group I of the periodic table with atomic number 55 and atomic mass 132.9054. There is one stable isotope 133 Cs, and 22 radioactive isotopes, among which 137 Cs with a half-life 27 years has found the broadest applications. Outer shell electronic conﬁguration is 6s 1 . Ionization energies are 3.893, 25.1, 34.6 eV. Atomic radius is 0.262; radius of Cs+ ion is 0.167 nm. Oxidation state is +1. Electronegativity is 0.68. Cesium is a silvery-white metal. It has a bodycentered cubic lattice with a = 0.605 nm (at 448 K). Density is 1.9039 g/cm3 (at 273 K) and 1.880 g/cm3 (at 300 K); Tmelting = 301.75 K; Tboiling ≈ 960 K. Heat of melting is 15.8172 kJ/kg, heat of evaporation is 613.2 kJ/kg; speciﬁc heat at constant pressure is 32.2 J·mole−1 ·K−1 at 298 K; thermal conductivity ratio is 16.7 to 27.2 W·m−1 ·K−1 at 301.6 K; linear expansion coefﬁcient is 9.7·10−5 K−1 (273 to 300 K). Electrical resistivity is 0.183 μ·m (at 273 K) and 0.2125 μ·m (at 300 K). Mohs hardness is 0.2; Brinell hardness is 0.015. Normal elastic modulus is 1.716 GPa at room temperature. Debye temperature is 42 K. Ion-plasma frequency is 1.724 THz; linear low-temperature electronic speciﬁc heat coefﬁcient is ≈3.20 mJ·mole−1 ·K−2 . Electronic work function of cesium polycrystal is ≈1.85 eV. Cross-section of thermal neutron trapping is 29 barn. Cesium is paramagnetic with magnetic susceptibility 0.1·10−6 (at 291 K).

Cesium is used in the production of photocells (it exceeds all the other metals in light sensitivity), of gas absorbers, and of low work function coatings for emitters. The application of “cesium plasma” is prospective for ionic reactor motors. CHAIN REACTIONS

Reactions of active particles (free radicals in chemical reactions, neutrons n in nuclear reactions), when the elementary interaction produces one or a number of additional active particles (radicals, A·). In the ﬁrst case the reaction is called an ordinary, non-branched chain reaction, in the second case it is a branched one. The chlorination process of H2 : Cl· + H2 → HCl + H·, Cl2 + H· → HCl + Cl·, . . . , etc., is an example of a non-branched chain reactions. The process of H2 oxidation represents an example of a branched chain reaction: H· + O2 → ·OH + O:, O: + H2 → ·OH + H·, ·OH + H2 → H2 O + H·, . . . , etc. In such a manner, the primary species A· may give rise to a large number (from ten to 107 ) of transformations of inactive particles (e.g., molecules). The number of such transformations per primary active species A· is called the chain length. The breaking of a chain (chain reaction termination) may be due to the presence of an impurity which interacts with A· so an additional A· is not produced. Also it may be due to the departure of A· from the reaction region. In the simplest situation (homogeneous case) the chain reaction rate is determined by the equation: v = K1 C1 P0 t × exp

(α − 1)K1 C1 − K2 C2 dt − βt ,

0

where P0 is the concentration of the primary species A· created by the initiating chain reaction, K1 and K2 are the velocity constants of chain reactions and the chain breaking reaction; C1 and C2 are the concentrations of initial substances of the chain reactions, and of the chain breaking centers; α is the number of A· species arising in the elementary act of chain initiation; β is a constant related to the probability of A· leaving the reaction region. The exponential term in this equation reﬂects the time change of the radical concentra-

CHALCOGENIDE MATERIALS

tion; and the relations between the terms in the exponent index determine the kinetic character of the chain reactions. So, if the ﬁrst term in the exponent index turns out to be larger than the sum of the others, then the chain reactions velocity increases exponentially with respect to time, and a chain explosion is possible. In solids chain reactions have been found in organic matrices. The matrix itself and also the components diluted in it can participate in these reactions. For example, in organic polymeric matrices which contain halide complexes of Au, Pt, Cu, Bi chain reactions can be initiated by the action of light or ionizing radiation on the system. As a result, atomic Cl· appears (e.g., [AuCl4 ]− +Cl· → [AuCl2 ]− +Cl2 +Cl·), and the chain length in such systems may reach 104 . The use of chain reactions for the photographic recording of information provides new opportunities for the creation of sensitive media with high resolution. Free radicals giving rise to chain reactions may be generated at the heterogeneous burning of solids and its mixtures in the reaction zone. In such a case the very existence these radicals determines the burning kinetics. There is some evidence that at burning, chain reactions also occur in the condensed phase. Nuclear chain reactions take place in uniform solid specimens of U-235 or Pu-239 (nuclear bomb), and also in the case of a nonuniform distribution of U-235 in some other material (graphite, heavy or light water, or of course U-239) which form the nuclear reactor. The ﬁrst nuclear chain reaction was realized by E. Fermi in 1942 in a uranium-graphite reactor. Up to the present time only uranium nuclear reactors are in use, and they satisfy the following conditions. The elementary act of ﬁssion involves a neutron n striking a U-235 nucleus in accordance with the reaction U-235 + n → A + B + kn + Q, where A and B are nuclear fragments (daughter nuclei), k is the neutron multiplication factor, and the chain reaction proceeds because the average value of k ∼ 2.5 for the elementary act of ﬁssion. The kn secondary neutrons in turn induce further ﬁssions The energy Q of the reaction is harnessed

163

in nuclear power plants for heating cities, producing electricity, etc. and the number of neutrons generated is greater than one (i.e. k > 1). The cross-section of the ﬁssion reaction of U-235 increases with the decrease of the neutron velocity v as 1/v, and there are resonances in the range of neutron energy from a fraction of an electronvolt to perhaps a hundred electronvolts. As a result, the so-called “thermal neutrons” play the main role in ﬁssion reactions. At these low energies the crosssection for the U-235 ﬁssion reaction is much larger than the cross-sections for other reactions with neutrons. Since there is a large probability that many neutrons will escape from a very small sample without reacting, there is a critical mass for the chain reaction to take place, and this is approximately 50 kg for U-235 and 10 kg for Pu-239. If the average neutron multiplication factor k is too large, the number of neutrons in the specimen can grow exponentially, leading to an explosion. To prevent this, neutron absorbing rods (e.g., graphite) are inserted into the reactor to remove excess neutrons and keep k ∼ 1 so the chain reaction will proceed slowly, and generate heat gradually. CHALCOGENIDE MATERIALS (fr. Gr. χαλκoς , copper and γ ενναω, engender)

Compounds of elements of Group VI of the periodic table (O, S, Se, Te, Po, collectively called chalcogens) with other elements. The class of chalcogenides (oxides, sulﬁdes, selenides, tellurides) contains the X−2 anion of Group VI elements. In view of their differences in properties and ﬁelds of application, oxides are often unfairly excluded from the list of chalcogenide materials, and polonium compounds are rarely included because they are strongly radioactive. In modern areas of engineering chalcogenide materials are often used in the form of thin lms or monocrystals, which are obtained through precipitation of aqueous solutions, decomposition of chelate compounds on a substrate, crystallization from gaseous (vapor) phase, etc. Typical ionic lattices of chalcogenides are characteristic of these elements, which exhibit very low values of ionization potentials. Many chalcogenide materials form lattices of the chalcopyrite type, the spinel type, and others. They are often nonstoichiometric compounds. Chalcogenides comprise a broad class of

164

CHANNELED PARTICLE FRICTION

compounds, including insulators, semiconductors and conductors of electric current. Chalcogenide materials are used in opto- and microelectronics, power engineering, in metallurgy, as photosensitive elements, transparent contacts, contactless switches, image converters, light indicators and electric phosphors, resistive salts, memory storage cells, etc. Historically the term chalcogenide was used for ores and minerals containing copper and sulfur: chalcopyrite (copper pyrite) CuFeS2 , the most important of all copper ores; chalcocite Cu2 S; chalcanthite CuSO4 ·5H2 O (blue vitriol), chalcostibite CuSbS2 , and others. CHANNELED PARTICLE FRICTION See Friction of channeled particles. CHANNELED PARTICLE SELF-ACCELERATION

A phenomenon observed during the passage of a beam of relativistic charged particles through a monocrystal in parallel to crystallographic planes or axes. Charged particles travelling in the channeling mode may radiate short-wave photons. By this action the channeling charged particles may absorb quanta emitted by other charged particles of the beam, and thereby increase their initial energy. Quasi-bound motion of charged particles in the planar or axial channneling mode may be regarded as one-dimensional or two-dimensional atoms. Thus in analogy with an atomic system, the process of self-acceleration of channeled particles may be called a quasi-Auger effect. For ultrarelativistic electrons entering a monocrystal parallel to crystallographic planes, the main radiation mechanism is electromagnetic quasi-characteristic radiation associated with the transitions of electrons from the free state to the channeling one. An electron in the quasi-bound channeling state may transfer to another quasi-bound state or escape into the continuum spectrum as a result of electron trapping (this exchange takes into account the possible contributions of not only real, but also virtual photons). The kinematics of this process shows that in the ﬁnal state it is possible to detect charged particles with double their initial energy.

CHANNELING in monocrystals

The transversely restricted (relative to the initial direction) motion of charged particles along open channels between neighboring close-packed atomic rows or planes in crystals. The condition for channeling is a small value of the angle subtended by the particle direction while entering the channel to the corresponding axis (for axial channeling) or plane (for planar channeling). This means that the particle being channeled experiences repeated glancing impacts with atoms of restraining chains (planes). These bend the trajectory in such a way that encounters with a small impact parameter become rare. The classical description of channeled ions proposed by J. Lindhard is based on using a potential averaged over the atoms of chains (planes), which is referred to as a string potential, or a continuous potential. In this case the angle ψ of the particle velocity vector relative to the axis of a chain or plane must be smaller than a critical value ψk = (U0 /E)1/2 , where E is the particle energy, and U0 is the height of the potential barrier created by the atoms of a chain or a plane. If ψ is greater than ψk , called the Lindhard angle, the particles are no longer conﬁned to the regime of channeling (see also Dechanneling). The manner of reﬂection of a particle from the walls of a channel suggests that a positively charged channeling particle spends most of its time moving past regions of a crystal with relatively low electron density. Therefore, the trapping of a particle into the channeling mode causes a reduction of its ionization energy loss and increases its effective mean free path in a monocrystal. In the channeling regime there is a considerable reduction of the probability of processes with small impact parameters relative to the sites of a crystal lattice (see Orientation effects). The occurrence of channeling was observed ﬁrst for positively charged ions, and later for electrons and positrons. It is of interest that the channeling phenomenon was “discovered” twice. In 1912, the German physicist J. Stark took notice of the fact that charged particles can penetrate to considerably greater depths along some preferential axes. However, this effect was forgotten for a long time until a “second discovery” in the early 1960s. It was found by computer

CHARACTERISTIC ENERGY LOSS

simulation that incident bombarding ions which have abnormally long paths through a monocrystal when they enter the crystal almost parallel to a main crystallographic direction. The channeling of relativistic charged particles gives rise to an intense electromagnetic quasi-characteristic radiation in the gamma ray and X-ray bands. See also Hyperchanneling, Molecule channeling, Neutral particle channeling, Quantum states of channeled particles, Okorokov effect, Channeled particle self-acceleration, Surface channeling, Surface conductive channel, Current lamentation. CHANNELING OF ION BEAMS

This takes place along the directions of atomic chains and planes in a monocrystal because the ions scattered at small angles to these directions cannot penetrate deep into the crystal (see Fig. 1). Shadow traces of the atomic chains and planes appear (the so-called shadow effect) at the target detecting the scattered ions. The emission of products of a nuclear reaction between the incident ions and the crystal atoms also produces the shadow effect. The shadow disappears, if the time

Fig. 1.

Fig. 2.

165

between the trapping of the ion nucleus by the crystal atom nucleus and the emission of the reaction product is long enough for the activated atom to displace noticeably from the blocking chain (plane). This allows one to estimate experimentally the nuclear reaction time. One can observe the blocking by the shadow effect resulting from the embedding of a radioactive isotope into a monocrystal. Fig. 2 shows the angular distribution of the intensity of emitted α-particles in a tungsten crystal upon the introduction of the 222 Rn isotope; the minimum corresponds to the 111 direction. Heating the crystal results in washing out the shadow due to thermal displacements of the atoms. CHARACTERISTIC ENERGY LOSS

Discrete energy losses, which are independent of the energy of incident primary electrons, and are characteristic of a given solid; they are observed in reﬂection and transmission spectra of secondary electrons. Characteristic energy loss is energy expended on the excitation of (i) electron transitions from inner core levels or from valence band levels to unoccupied levels, vibrational energy levels, and (ii) collective longitudinal oscillations of a solid-state plasma (plasmons). The values of characteristic energy losses of the ﬁrst kind (30–105 eV) are easily determined from the binding energies (Eb ) of electrons in atoms, and are used in ionization spectroscopy for the analysis of solids. Different solids exhibit different binding energies because of many-particle effects (relaxation, multiplet splitting, con guration interaction, shake-off and shake-up, chemical shifts). Characteristic energy losses of the second kind (1–30 eV) are more difﬁcult to interpret, since they are due to processes involving levels of the valence band and upper unoccupied levels. Vibrational characteristic energy losses are related to transitions between the vibrational states of surface atoms (molecules) of a solid, or of adsorbed layers; these characteristic energy losses are a source of information on phonon involvements. Volume and surface plasmon characteristic energy losses (ωP and ωS , respectively) are determined by the concentration of valence electrons n: ωP = (4πe2 n/m)1/2 , √ ωS = ωp / 2, and they manifest themselves

166

CHARACTERISTIC ENERGY LOSS SPECTROSCOPY

as distinct lines in the spectra of materials with weakened valence electron bonding. Other materials (e.g., transition metals) exhibit diffuse plasma characteristic energy loss lines. See also Characteristic energy loss spectroscopy. CHARACTERISTIC ENERGY LOSS SPECTROSCOPY

Branch of physics concerned with the discrete energy losses that are experienced by a monochromatic primary electron beam interacting with a solid. Characteristic energy loss spectroscopy examines samples using either the transmitted beam or the reﬂected beam of light. The techniques are applied to the investigation of inner core levels in atoms of solids, shifts of these levels caused by changes of the chemical environment, electron transitions from valence band levels to unoccupied levels, transitions among vibrational states of atoms of adsorbed layers at solid surfaces, generation of collective longitudinal plasma oscillations (plasmons). These studies provide information on the composition and electronic properties of the material as a whole, and in particular of its surface. The major ﬁelds of application are the spectroscopy of surface plasmons and vibrational characteristic energy loss spectroscopy, which allows one to perform a complete analysis of the surface. As distinct from optical spectroscopy, vibrational characteristic energy loss spectroscopy affords: (1) operation over a broad energy band (0.001–1 eV), which includes phenomena inaccessible by optical methods; (2) excitation of optically forbidden transitions, and (3) an increase of the scattering cross-section. There exists the following classiﬁcation of spectroscopic methods according to the type of physical process involved in the energy losses: ionization spectroscopy of valence and inner core levels, plasmon characteristic energy loss spectroscopy and high-resolution vibrational spectroscopy. The intensity of spectral lines due to characteristic energy losses is not very high, and decreases with an increase of the probing beam energy; therefore, electrons with energies below 2 keV are used, so the probing depth in this case does not exceed 2 nm. Thus, characteristic energy loss spectroscopy is the preferred method for examining near-surface layers of solids.

CHARACTERISTIC LENGTH OF MAGNETIC MATERIAL

Parameter lw of uniaxial magnetic materials, with the dimensionality of length, which is equal to the ratio of the surface energy density of a Bloch domain wall to the maximal volume energy density of the demagnetization eld μ0 M 2 /2. In materials with a quality or Q-factor (see Magnetic lms) exceeding 1 the characteristic length determines the minimal diameter of a magnetic bubble domain (or minimal spacing of the band domain structure), that may occur in thin layers (ﬁlms) along the easy magnetization axis, which is perpendicular to the developed surface. The largest possible diameter of an isolated magnetic bubble domain is ≈3.9lw , and the layer thickness in this case must be ≈3.3lw . CHARACTERISTIC LENGTHS IN SUPERCONDUCTORS Coherence length ξ , penetration depth of magnetic eld λ, length of imbalance relaxation λE (see Penetration depth of electric eld), Josephson

penetration depth. The superconducting phase transition is characterized by the generation of bound states, i.e. Cooper pairs of electrons which are bosons, and are subject to Bose–Einstein condensation. The coherence length ξ is the effective radius of a Cooper pair, and it determines the characteristic distances over which the complex order parameter of the superconductor ψ(r) (effective wave function of Cooper pair) changes to an appreciable extent when the superconductor is in a certain nonequilibrium state; e.g., at the penetration of Abrikosov vortices into a superconductor (ξ is the radius of the normal state vortex core), at the interface of a superconductor with a normal metal (proximity effect), etc. Typical values of ξ range from 10−6 m in pure metals to 10−9 m in alloys and compounds. The coherence length of a pure (type I) superconductor is ξ0 = vF /π 0 , and in the case of a (type II) superconducting alloy with electron mean free path ll , which is small compared with ξ0 , the coherence length at the temperature 0 K is of the order of ξ(0) ≈ (ξ0 ll )1/2 . In the neighborhood of the transition point, ξ tends to inﬁnity as ξ(T ) ≈ ξ(0)/(1 − t)1/2 , where

CHARACTERISTIC SURFACE

t = T /Tc . In a type II superconductor, the magnitude of ξ is related to the value of the upper critical e ld Bc2 through the expression Bc2 = Φ0 /(2πξ 2 ) (Φ0 = h/(2e) is the ux quantum). The Meissner effect in superconductors arises from the fact that external magnetic ﬁeld creates a current (Meissner current) in the surface layer which screens the bulk of the superconductor from the penetration of the ﬁeld. The characteristic thickness of this layer is called the penetration depth λ. In the case of a pure type I superconductor, the London penetration depth is determined from the London formula λ0 = [mc2 /(4πne2 )]1/2 and is of the order of 10−7 m. In the case of a superconducting alloy, λ > λ0 , with the value λ ≈ λ0 (ξ0 / ll )1/2 at ξ0 ll . In the neighborhood of Tc , λ has the temperature dependence λ(T ) ≈ λ(0)/(1 − t)1/2 . The penetration depth λ may be determined experimentally from the change of the superconductor inductance, which is due to partial penetration of the ﬁeld into the bulk of the solid. The imbalance relaxation length λE determines the characteristic distances of nonequilibrium processes in superconductors. The simplest case is the current ﬂow through a galvanic contact between a normal metal and a superconductor. In the normal metal, the current is carried by electrons, whereas in the superconductor it is carried by Cooper pairs. The conversion of normal excitations into pairs in the normal metal takes place at the distance λE from the interface. The electric ﬁeld E differs from zero in this region, therefore λE may be considered as the depth of penetration of a longitudinal (in contrast to the Meissner effect) “dissipative” electric ﬁeld. The nonequilibrium state of the superconductor exists within the distance ∼λE of the interface. This state is characterized by an imbalance in the occupancy of electron-like (P > PF , where PF is the Fermi momentum) and hole-like (P < PF , where P is excitation momentum) spectrum band branches. The imbalance relaxation is related to inelastic collisions (i.e. electron–phonon types), characterized by a mean free path length lε = vF τε , which are inefﬁcient at low temperatures, and therefore lead to rather high values of λE (e.g., λE ∼ 10 μm). According to theory, λE = (DτQ )1/2 , where D = vF ll /3 is the electron diffusion coef cient,

167

and τQ = [4T /(πΔ)]1/2 τε is the period of the imbalance relaxation. In the neighborhood of Tc , λE varies as λE (T ) ≈ λE (0)/(1 − t)1/4 . The value of λE determines the characteristic dimensions of the region of inhomogeneity (so-called phase slip centers) in the resistive state of superconducting ﬁlms. The Josephson penetration depth has the value λJ = [Φ0 /(2πμ0 Jc deff )]1/2 where Jc is the critical current and deff is the effective thickness of the junction. A Josephson junction is considered short when its length is less than λJ , and it is long when it has a greater length. CHARACTERISTIC SURFACE, ellipsoid

A second-order surface, which represents the orientation dependence of a particular physical property of a crystal, which is described by a second-rank tensor. The equation of the characteristic surface, when reduced to the principal axes of the crystallophysical coordinate system (e.g., an orthogonal crystal coordinate system compatible with nonorthogonal lattice constant directions) is of the form s1 x12 + s2 x22 + s3 x33 = 1, where s1 , s2 and s3 are the principal values of the tensor sij . If all sii are positive, then the characteristic surface is (in the general case) a three-axis ellipsoid; with its semiaxes equal, respectively, to (s1 )−1/2 , (s2 )−1/2 and (s3 )−1/2 , and proportional to the values of the particular physical property represented by the sij in question along the principal axes. For a random direction, speciﬁed by radius vector r, we have rij = (sij )−1/2 . In accordance with the Neumann principle (which states that the symmetry group of a certain physical property of a crystal must include the symmetry elements of the point group of the crystal), the symmetry of the characteristic surface corresponds to the symmetry of the physical property. For all positive values of sii the characteristic surface is a sphere for cubic crystals which belong to the highest symmetry category. The characteristic surface of the crystals which belong to the medium category, those with tetragonal, hexagonal or trigonal structures, has the shape of spheroid (prolate or oblate ellipsoid), whereas

168

CHARACTER OF GROUP REPRESENTATION MATRIX

crystals of the lowest symmetry category which are orthorhombic, monoclinic, or triclinic, are described by a characteristic surface in the form of a three-axis ellipsoid. An example of a characteristic surface associated with optical anisotropy represents the dependence of the refractive index n on the direction in the crystal; depending on the shape of this surface crystals are classiﬁed as optically isotropic, uniaxial crystals or biaxial crystals. The main property of the characteristic surface may be stated as follows: if vectors A and B are interconnected by the relation Bi = sij Aj and the radius vector r of the characteristic surface tensor sij is parallel to the vector A, then the direction of the vector B coincides with the normal to the plane, which is tangent to the characteristic surface at the contact point of the vector r. Characteristic surfaces apply in the linear or harmonic response range of physical properties. Besides the characteristic surface, the concept of an indicating surface is sometimes introduced: x12 s12

x2 x2 + 22 + 32 = 1. s2 s3

Radius vectors, which terminate at this surface, designate the absolute values of the physical properties in a given direction. CHARACTER OF GROUP REPRESENTATION MATRIX

The trace or sum of the diagonal elements of a group representation matrix. The character is independent of the choice of coordinate system, and all irreducible representations of the same class have the same character. The character table of the irreducible representations has orthogonality properties (see Group theory). CHARGE CARRIER DRIFT See Current carrier drift. CHARGE COUPLED DEVICES

A broad class of devices (charge transfer devices, charge coupling devices, and related chargeinjection devices) that allows for the scanning of an optical image in a manner similar that of a cathode ray tube (vidicon). The main purpose of such devices is the transmission of TV signals of various spectral bands: they are also used

in random-access memories. The mechanism of charge coupling action can, to some extent, be represented by a combination of a bipolar transistor (motion of minority current carriers) and a eld-effect transistor (controls carrier motion by changing displacement voltage at the gate). The electrodes (gates) have a mosaic structure, and the distance between the edges of adjacent elements does not exceed the diffusion length of nonequilibrium carriers. The application of a bias voltage to a single gate element creates a “potential well” under this element for minority carriers. The latter accumulate under the gate in quantities proportional to their rate of generation. In a two-dimensional array of such elements, each “operating element” with the bias that corresponds to the accumulation of minority carriers has unbiased elements as neighbors on every side. Upon supplying the bias to an element adjacent to the operating one, a “potential well” appears under it. If the well is deep enough the packet of minority carriers from the “operating element” well moves into it. The sequence of voltage pulses at the gate elements is set so that the packet shifts by the length of one element with each pulse, thus the charge of every “operating” element can be led sequentially through to the output element, producing an output signal proportional to this charge. CHARGE DENSITY OSCILLATIONS See Plasma oscillations. CHARGE DENSITY WAVE in metals

Periodic redistribution of electronic, ionic and total charge in space, caused by small periodic displacements of ions near their equilibrium positions in the crystal lattice. The charge density wave (CDW) state is detected via the scattering of X-rays, fast electrons and neutrons, which exhibits diffraction peaks from the source lattice and weaker peaks from their “satellites” (see X-ray structure analysis, Electron diffraction analysis). A charge density wave can appear when the metal is cooled below some critical temperature. The phase transition to the CDW state is characterized by changes in the temperature dependence of the resistance, Hall constant, magnetic susceptibility, and a modiﬁcation of the electronic spectrum of the metal. The charge density wave

CHARGED PARTICLE ENERGY LOSS

period can be commensurate with the period of the source lattice, and in these cases one can talk about commensurate CDWs which differ from incommensurate ones. As a rule in the cases of incommensurability the lattice period depends on the temperature, and structural transitions to the commensurable CDW are possible. The transition to a charge density wave state is found in metals with strong anisotropy of the electronic spectrum. This anisotropy can have a two-dimensional character, when the electrons move freely in a plane (their Wannier wave functions at different points overlap), but between the planes their motion is restricted (due to the weak overlapping of the electronic Wannier functions). Related to such compounds are, e.g., the layered compounds of dichalcogenides of transition metals like TaS2 , NbSe2 (see Quasi-two-dimensional crystals). Anisotropy of a one-dimensional type is realized in compounds with a chain structure, e.g., in organic conductors (see Quasi-one-dimensional crystals). The origin of transitions to the CDW state for all these systems is associated with the features of the geometry of the Fermi surface. The theory shows that if sufﬁciently large sections of this surface are nested, meaning that they are can be overlapped with each other by translation along a reciprocal lattice vector Q, then the polarizability of the system of electrons in the periodic electric ﬁeld of the lattice E = Re (E0 eiQr ) (r is the radius-vector of the lattice point) is high and the lattice becomes unstable with respect to the appearance of periodic distortions with wave vector Q. The distortions are formed below the critical temperature and cause an energy gap to appear in the electronic spectrum at the nested sections of the Fermi surface, i.e. with the complete or partial loss of metallic properties. The degree of nesting, as well as the extent of the metallic property loss grows with increasing anisotropy of the electronic spectrum. In quasi-two-dimensional (layered) compounds the appearance of an energy gap at the whole Fermi surface is impossible, and they preserve their metallic properties at transitions to CDW state, or in case of large displacements of atoms they become semimetals. In quasi-one-dimensional compounds the region of Fermi surface nesting is more extensive, and the

169

energy gap may occur on the whole Fermi surface. Then quasi-one-dimensional compounds in a state with a charge density wave become insulators (see Peierls transition). CHARGE DENSITY WAVE IN SUPERCONDUCTOR See Superconductor with charge (spin) density waves. CHARGED PARTICLE ENERGY LOSS in a solid

This loss occurs during the interaction of incoming charged particles with atoms and electrons of a target. It is characterized by the average braking ability equal to −dE/dx, where E is the particle energy and coordinate x is its initial direction, and by straggling of the charged particle energy loss (by the root mean square scattering of the energy loss value). This energy loss determines the values of charged particle path in the material. Calculation of the energy loss is a complex many-particle problem, and to solve it requires the adoption of a series of approximations which differ for high- and low-energy particles, for long-range and short-range collisions, and also for the different correlations of masses and charges of interacting particles, taking into account the so-called density effect associated with the polarization of the medium by the ionizing particle, of the resonance recharging of the moving ions, etc. The main mechanisms of charged particle energy loss are the nuclear decelleration or braking caused by elastic collisions (taking place without variation of internal energy), collisions of atoms (ions); electron braking caused by the inelastic collisions leading to the excitation and ionization of the atomic electron shells, and also of the free electrons of the irradiated material (see Characteristic energy loss). Besides, there is the charged particle energy loss from radiation – Bremsstrahlung and Cherenkov radiation; the loss is substantial for light particles, especially for electrons and positrons. The value of this loss depends on the energy, charge, and mass of the moving particles, as well as on the charge, mass, and density of the target atoms. For motion close to the direction of low-index crystallographic axes and planes, the energy loss strongly depends on the direction of the incident beam (see Orientation effects; Channeling); in other cases the target may

170

CHARGED PARTICLE PATHS

be approximately considered as an amorphous one with isotropic loss. In the approximation of the Lindhard–Scharf–Schiott theory charged particle energy loss of ions in an amorphous medium is expressed in terms of dimensionless variables for the energy ε = aEM2 /[e2 Z1 Z2 (M1 + M2 )], and coordinate ρ = 4πxa 2 NM1 M2 /(M1 + M2 )2 , where M and Z are the masses and atomic numbers of the incident ions (subscript 1) and of the atoms of the medium (subscript 2), N is the density of the atoms of the medium, 2/3 2/3 a = 0.8853aB (Z1 + Z2 )−1/2 , aB is the Bohr radius. Taking into account the structure of the atomic electron shells supplements the results of the Lindhard–Scharf–Schiott theory concerning an oscillating (within limits of tens of percents) dependence of dE/dx on Z2 caused by the contribution of the valence atomic shells to the charged particle energy loss of the electrons. The charged particle energy losses of positrons and electrons of not too high energies E < Ecr when the role of braking radiation is not yet appreciable, are determined by nuclear and electron braking, with values having qualitative regularities close to the charged particle energy loss of ions, but differing from the ion values mainly due to the mass difference between the electrons (taking into account relativistic corrections) and ions. The value of Ecr may be evaluated from the correlation Z2 Ecr [MeV] ≈ 800. For different energy ranges, masses, particle charges, and target parameters, there are different approximations for the calculation of the charged particle energy loss, and there are also many available experimental data. CHARGED PARTICLE PATHS in condensed media

Characteristics of charged particle trajectories that are limited by the charged particle energy loss during collisions with atoms and electrons of the medium. The particle path in a medium is a broken line since each collision results in a change of particle momentum and direction. The total vector path, R, is the distance between the particle entry point and its terminal point where it has already expended most of its energy and stopped. The projective path Rp presents a projection of R onto the direction x of the initial

particle momentum (e.g., the latter may be normal to the bombarded plane, yz). The transverse path R⊥ characterizes the change of the initial coordinate of the particle in the yz plane at the time the particle stops. Finally, one may consider the total or effective path RL which is equal to the full length of the distance travelled by the particle taking into account all deviations from a linear track. The number of particle collisions per unit path length, the impact parameters for each collision, and, hence, the trajectory of each individual particle are probability variables, even for identical initial conditions of particle motion, so there exists a certain distribution of charged particle paths over their lengths. When bombarding a sample with a beam of ions of the same chemical element with equal initial energies the proﬁle of stopped ions appears to exhibit a certain broadening. Such a distribution is often characterized by the moments M1 = Rp = x; M2 =

Rp2 = (x − x)2 , . . . , Mk = (x − x)k (k = 3, 4, . . .), x k = (r cos θ)k p(r, θ; E) dr, where p(r, θ; E) is the probability for a particle entering the crystal with energy E at the zero coordinate point along the direction n to stop at point r, so that θ = arccos(nr/r). The value

Rp presents the statistical average scatter (straggling) of particle paths, M3 that is a measure of distribution asymmetry. The accepted measure of asymmetry is the so-called distribution skewness, 3/2 Sk = M3 /M2 . In the case of Sk < 0, the path distribution falls off more sharply from its maximum in the bulk sample, and when Sk > 0 a sharper fall-off is at the surface of the sample. The pathways become longer in the case of channeling. Electron pathways in the medium typically feature much sharper trajectory breaks compared to the pathways of heavy particles. Because of multiple collisions, the electron quite soon “forgets” its initial direction of propagation. Moreover, electrons penetrate the medium in a diffusion manner. To retrieve the pathways experimentally electrons of varying initial energies are shot through thin plates. The maximum plate thickness at which a throughput electron current is still recorded corresponds to the maximum path length for an electron with a given energy penetrating the material. A normal pathway is one with a plate thickness

CHEMICAL BONDS

such that the initial electron beam intensity decays by a factor of 6 when passing through it. An empirical dependence for electrons with initial energies E 0.6 MeV is Rp [mg/cm2 ] = 526E[MeV] − 94. CHARGE, MAGNETIC See Magnetic charge. CHARGE-TRANSFER COMPLEXES

Organic compounds consisting of molecules of two types: one acts as an electron donor and the other as an electron acceptor, the charge being redistributed between the neighboring donors and acceptors. Charge-transfer complexes have an electric dipole moment even if they are created from nonpolar molecules, and they exhibit paramagnetic properties, whereas the initial donor and acceptor molecules are diamagnetic. If an electron in the ground state of the organic solid is completely transferred from donor to acceptor, such a compound is called an ion-radical salt (limiting bond case in charge-transfer complexes). Besides weak charge-transfer complexes of ion-radical salts, there are many such compounds with intermediate strength bonds. The properties of chargetransfer complexes are strongly dependent on the extent of charge transfer, and on the magnitude of the donor–acceptor interaction. The electrical conductivity of these complexes at room temperature varies over a wide range: from 10−15 up to 102 –103 −1 ·cm−1 . The temperature dependence of the electrical conductivity is of the semiconductor type; hence, most charge-transfer complexes are organic semiconductors. These are exempliﬁed by compounds of different molecules with the molecular acceptor tetracyanoquinodimethane (TCNQ). Because of the strong acceptor properties, the planar structure, and the high symmetry of the TCNQ molecule, one can obtain charge-transfer complexes with a rather high conductivity (as high as 104 −1 ·cm−1 ). A large variety of organic charge-transfer complexes have been synthesized that exhibit properties ranging from those of semiconductors to metals and superconductors (see Superconductivity). The latter two categories include mainly ion-radical salts. Molecular charge-transfer complexes are of interest as photosemiconductors (see Photoconductivity).

171

CHEMICAL BOND PREDISSOCIATION The state of a chemical bond, usually an ex-

cited one, having an energy that exceeds the energy of atoms in the dissociated state. The latter is separated from the initial state by a barrier which may be overcome by tunneling (see Tunneling phenomena in solids). The simplest example of chemical bond predissociation is the excited hydrogen molecule H2 with a dissociation energy ≈4.4 eV, whereas the excitation energy upon transition of one of the atoms to the level 2p is ∼10 eV. Another example is the state of an α-particle in a radioactive nucleus, e.g., of Ra or U, whose average lifetime is, respectively, 1600 and 4.4·109 years. CHEMICAL BONDS in solids

Bonds between atoms of a solid; isolated atoms decrease their free energy during the redistribution of their electron densities when they join together through chemical bonding. The nature of a chemical bond is determined by the nature of the constituent atoms, and by the type of structure adapted by the solid. There exist molecular crystals, whose structural elements are molecules; under evaporation this crystal type decomposes into molecules. Crystals can be formed from monatomic molecules of noble gases (He, Ne, Ar, Kr, Xe, Rn), diatomic molecules (H2 , O2 , NO, CO), triatomic molecules (H2 O, H2 S, NO2 ), and molecules of a more complex composition (NH3 , CH4 , etc.). In these cases every molecule has saturated bonds, and the attraction of molecules toward each other is through van der Waals forces or hydrogen bonds, as in H2 O, H2 S, NH3 . A certain (additional) role is played by Coulomb forces, if the atoms have a partial charge, as, e.g., in CO2 and H2 O molecules. In cases when the molecules contain atoms of Groups I, II, III, together with those of Groups V, VI, VII of the periodic table, i.e. they are polar molecules, then Coulomb forces become dominant to the extent that individual molecules are not observed in the crystal, and its structural elements are ions. Typical examples are provided by alkali-halide crystals, and oxides of alkaline earth metals. In these compounds every ion is usually symmetrically surrounded by ions of opposite sign (six for FCC NaCl, eight for BCC CsCl); and the stronger ionic bond is formed. For these cases the

172

CHEMICAL DIFFUSION

action of van der Waals forces between ions becomes of secondary importance. The opposite case is provided by crystals of elements of Group IV: diamond, silicon, germanium, gray tin. There are no charges on the atoms of these crystals, and the formation of covalent bonds, or homopolar bonds, is due to the sp3 -hybridization of orbitals (atomic orbitals), and to the attraction of electrons to the nuclei (skeletons) of neighboring atoms. As only four hybrid orbitals may be formed by a combination of s- and p-orbitals, the number of closest neighbors (coordination number) for these crystals is limited to four. Each atom of one sublattice is tetrahedrally surrounded by four atoms of the other sublattice. The binary A(n) B(8−n) type crystallization of elements (sphalerite lattice) is formed analogously, e.g., BN, GaP, ZnS, HgTe, CuCl. However, the atoms of the metal and the metalloid in these compounds possess fractional charges of opposite sign, with the metal atom positively charged. This is a combined (hybrid) polar-covalent bond (ionic-covalent bond). The smaller the number n of the periodic table group, the more ionic the bond. In metals and alloys the so-called metallic bond also occurs: it is formed through delocalization of valence electrons. At the formation of the crystal the outer (valence) s- and p-electrons (elements of Groups I to III, and transition elements) leave their atomic nuclei and migrate between ions over the entire lattice. As this takes place, their kinetic energy decreases (in accordance with the uncertainty relation). It is this energy decrease that is responsible for the formation of a metallic bond; alkali metals and alkaline earth metals possess relatively weak metallic bonds (1 to 2 free electrons per atom), whereas elements such as Fe, Ti, Pt exhibit rather strong metallic bonds. For a fairly broad class of hydrogen-containing organic compounds there is a noticeable contribution to the crystal formation energy from hydrogen bonds. Typical examples are provided by ice, solid ammonia, and the ferroelectric crystal KH2 PO4 . Because of its comparatively small mass, a positively charged hydrogen atom exhibits quantum behaviour and spends some time near an electronegative atom (see Electronegativity) of one of the neighboring molecules, which results in a decrease of the overall system energy. Many solids

exhibit several types of chemical bonds, usually with one or two bonding types dominant. CHEMICAL DIFFUSION The same as Heterodiffusion. CHEMICAL HEAT TREATMENT Heat treatment in a chemically active medium

involves the diffusive saturation of a metal surface with chemical elements of the medium. Both nonmetals (B, C, N, etc.) and metals (Al, Ti, Cr, Zn, etc.) are used as diffusible elements. In a number of cases simultaneous saturation with metals and nonmetals is used, including multicomponent saturation. During chemical heat treatment a diffusion layer is formed as a result of prior processes of dissociation in the active external medium, adsorption of dissociated atoms on the surface of the base metal, and diffusion of the saturating element. Chemical reactions bring about dissociation with the generation of active atomic states of chemical elements (e.g., ammonia decomposition under nitriding). Adsorption of dissociated atoms may take place either through the action of van der Waals forces of attraction, with the generation of an adsorption layer (physical adsorption), or because of chemical bonding with atoms of a metal surface (chemisorption). Simultaneously with these processes, the main chemical heat treatment process goes on, namely the diffusion of adsorbed atoms into the depth of the metal. The result is the formation of a diffusion layer with a certain distribution of diffusible elements relative to the depth. The concentration changes monotonically with depth, so a continuous sequence of solid solutions forms with the base metal. The chemical composition of the layer is more complicated if the solid solutions have limited solubility, or if chemical compounds form. In this case the layer includes different phases, in accordance with the phase diagram of the saturating element with the base metal at the diffusive saturation temperature, and the concentration dependence on the depth can undergo abrupt changes. The duration of diffusive saturation is determined by the depth of the diffusion layer, which increases quadratically with time. The main methods of chemical heat treatment with respect to the type of active medium are: saturation from powders and

CHEMICAL SHIFT

pastes, gaseous media, melts of metals and salts, as well as evaporation of the diffusible element in vacuo. Chemical heat treatment involving a single element includes nitriding, aluminizing, boronizing, siliconizing, titanizing, zinc plating, cementation. Saturation with two elements takes place at aluminoboronizing, aluminosiliconizing, chromosiliconizing, nitrocementation, cyaniding. This treatment involving several diffusible elements includes saturation with boron and silicon together with other metals (Ti, Cr, Mo, W, etc.), as well as saturation with aluminum and chromium together with other metals (Ti, V, Mn, Zn, etc.). Chemical heat treatment is used in industry to increase the reliability and service life of metallic working parts of devices and engines. Depending on the chemical composition of the metallic work piece and the nature of the saturating elements, treated articles may acquire increased hardness, strength, corrosion resistance and cavitation resistance, wear resistance (see Wear), etc. CHEMICAL METHODS OF ANALYSIS

Methods of analysis based on the use of chemical reactions. Methods of quantitative analysis involve the determination of the masses of the reaction products (gravimetry); determination of the volume of the solution of one substance required to react quantitatively with a given solution volume of another substance (titration analysis), determination of thermal effects of the reaction (calorimetry), of its rate (kinetic methods), etc. Methods of qualitative analysis are based on carrying out chemical reactions, which indicate either the presence of ions of certain type in the solution, or the presence of certain atoms in organic compounds. Chemical methods of analysis have been largely superseded by more accurate physical and physicochemical methods of analysis. CHEMICAL POTENTIAL (introduced by J.W. Gibbs, 1873–1878)

Thermodynamic state function, which deﬁnes the change of thermodynamic potential for the change in the number of particles of the ith type Ni in open multicomponent systems with varying numbers of particles, which are described by the grand canonical distribution (see Gibbs distributions). The chemical potential μ of the ith

173

component equals the partial derivative of every thermodynamic potential (e.g., Helmholtz free energy F ) with respect to Ni while holding other thermodynamic quantities constant (e.g., μi = ∂F /∂Ni at T = const, V = const and Nj = const for j = i). The chemical potential for constant pressure conditions is closely related to Gibbs free

energy G = i μi Ni , and in the case of a singlecomponent system μ = G/N , i.e. the chemical potential is equal to Gibbs energy per particle. For quantum systems of bosons, which obey Bose–Einstein statistics, the chemical potential is negative at temperatures higher than the Bose– Einstein condensation temperature T0 , and is equal to zero below T0 , and in systems with varying numbers of particles (phonons in solids, photons in equilibrium with thermal radiation). For a system of fermions, which obey Fermi–Dirac statistics, the chemical potential is positive at temperatures below the degeneracy temperature (Fermi temperature) TF , it coincides with the Fermi energy EF at absolute zero of temperature; and for T > TF the chemical potential satisﬁes the inequality μ < EF . In external potential ﬁelds (gravitational, electric) the role of the chemical potential is played by the quantity μi = μ0i + Ui (r) = const, where μ0i is the chemical potential in the absence of the ﬁeld, and Ui (r) is the potential energy of particles of the ith type in the external ﬁeld. For charged particles in an electrostatic ﬁeld E = −∇ϕ(r) the expression for the electrochemical potential μi = μ0i +ei ϕ(r) = const holds true. Equal values of chemical potential in different phases deﬁne equilibrium conditions for phase equilibria (the so-called Gibbs’ phase rule) and chemical reactions. The chemical potential in a solid determines the electronic work function of a crystal for e ld electron emission, thermionic emission and photoelectron emission, electron af nity, contact potential difference, and other properties. CHEMICAL SHIFT

Term used to describe changes (depending on the speciﬁc nature of the material under investigation) of the positions of energy levels or spectral lines which can arise from the local electronic or chemical environment. The values of chemical

174

CHEMILUMINESCENCE

shifts are usually given as parameters corresponding to the spectrum (energy state) of a given material. Generally the chemical shift is measured either in the same units as the basic quantities which characterize the spectrum, or in dimensionless units. The term is most widely used in high resolution nuclear magnetic resonance (NMR) spectroscopy, in Mössbauer spectroscopy, in the physics of semiconductors to describe the location of impurity energy levels, etc. In high-resolution NMR the chemical shift is the shift of the resonance signal. The mechanism producing this shift is as follows: an atom (molecule) is placed in an applied magnetic ﬁeld B 0 ; and as a result of Larmor precession of electrons oriented parallel to and antiparallel to B 0 the ﬁeld B ∗ arises (see Diamagnetism), so the nucleus experiences the action of an effective magnetic ﬁeld B = B0 − B ∗ = B0 (1 − σ ), where σ is called the screening constant; usually σ ∼ 10−6 . For nuclei of a given type, which are in different electronic surroundings, i.e. either in different molecules or at nonequivalent sites of one molecule, the resonance will be observed for different values of B0 (at a given frequency). In practice the NMR chemical shift is measured in relative units δ = (B − Bst )·106 /B0 , where B and Bst are the respective resonance values of the external ﬁeld for the sample under investigation and a standard substance. The chemical shift is one of the main characteristics of high resolution NMR spectra, which are observed for liquids (and occasionally gases). The value of this shift provides information on the electronic structure of molecules, and the nature of chemical bonds. The development of a recent trend in spectroscopy, namely highresolution NMR spectroscopy of solids, permits the measurement of chemical shifts in solids. In the Mössbauer effect the chemical shift (also called isomer shift) makes its appearance if the source and absorber differ chemically. In the physics of semiconductors a chemical shift manifests itself in the difference between the energy states of impurity levels, expressed in terms of the effective mass, and the energy states calculated from theory, taking into account corrections to the potential due to the speciﬁc atom (ion). For example, some donor levels exhibit fairly large

chemical shifts in their ground state energies due to correlation and exchange effects involving the donor and core electrons. CHEMILUMINESCENCE Luminescent excitation that results from chem-

ical reactions. The process of chemiluminescence involves the emission of radiation either by products of a chemical reaction, or by other components which become excited by absorbing energy transferred to them from reaction products. Chemiluminescence in solids arises at a boundary with a gaseous or liquid phase as a result of heterogeneous reactions (see Heterogeneous system), which proceed either spontaneously (intrinsic chemiluminescence) or under action of various external factors: e.g., electrical, electrolysis (electroluminescence). A speciﬁc case of chemiluminescence is bioluminescence (e.g., luminescence of rotten wood). Chemiluminescence constitutes the basis of action of chemical lasers, and is used for the analysis of gases and solid surfaces. CHEMISORPTION, chemical adsorption

Chemical binding of particles of a substance (atoms, molecules, radicals) by a solid surface. It differs from physical adsorption by its stronger bonding, that is by a higher value of the binding energy (0.5–10 eV). The bond between the adsorbed particle and the solid can have both covalent and ionic components; the former due to overlap of the electronic wave functions of the adsorbed particle and the substrate atoms, and the latter due to the transfer of charge from the adsorbed particle to the solid material. An adsorbed ion in conjunction with charges which screen it can form a dipole, which results in the adsorbed ﬁlm changing the electronic work function of the solid. Particles chemically adsorbed on the surface of a solid interact with one another, and sometimes generate an ordered two-dimensional lattice of adatoms (see Monolayer). Chemisorption plays an important role in the oxidation of metals, heterogeneous catalysis, crystal growth, electronics, etc. CHEMISTRY See Crystal chemistry, High-energy chemistry, Mechanochemistry, Mesonic chemistry, Quantum chemistry, Radiation chemistry, Solid state chemistry.

CHIRALITY OF MAGNETIC BUBBLE DOMAINS

CHERENKOV RADIATION (S.P. Vavilov, P.A. Cherenkov, 1934); referred to as Vavilov–Cherenkov radiation in the Russian literature Photons emitted by charged particles moving

in a medium with a speed v which exceeds the speed of light u = c/n in this medium, where n is the refractive index. In condensed matter with high values of n Cherenkov radiation is observed at electron energies of about 105 eV, and at protons energies of 108 eV. This radiation is explained via Huygens principle by noting that waves which are emitted at points along the charged particle trajectory for the condition v > u will overtake waves emitted earlier by the particle. As a result of their interference, a light cone is formed having a vertex that coincides with the instantaneous position of the emitting particle, with θ the angle between the direction of the particle’s movement and the direction of propagation of the outgoing radiated wave satisfying the relation cos θ =

1c . nv

The spectral distribution of energy E(ω) for Cherenkov radiation is determined by the relation dE c2 e2 = 2ω 1− 2 2 dω c v n for the condition v > c/n(ω). There is no radiation for frequencies ω which do not satisfy the above condition. Cherenkov radiation has found wide application in Cherenkov counters used for determining the speeds, charges, and masses of fast charged particles (electrons, positrons, mesons, protons, and antiprotons); and for studying optically anisotropic media, including waveguides. CHI PHASE (χ -phase) An intermetallic compound with a cubic lattice

isomorphic to that of cubic α-Mn. It is formed mainly by transition metals. The best known chi phases are those involving rhenium with refractory materials. In alloys of rhenium with molybdenum, tungsten, niobium and tantalum the chi phase contains about 75 at.% Re. In the systems Mo–Re and W–Re the chi phase is obtained by the peritectic reaction (see Peritectic alloys) at 1850 ◦ C

175

in the system Mo–Re and at 2150 ◦ C in the system W–Re; and this reaction only takes place for a narrow region of homogeneity. In the systems Nb–Re and Ta–Re the χ -phase melts without decomposition and exhibits a broad range of homogeneity. In systems formed by Re with Ti, Zr and Hf the composition of the χ -phase is approximately Me5 Re24 ; it is formed by the peritectic reaction, and has a moderate range of homogeneity (Me–Ti, Zr or Hf). The chi phase has also been observed in binary systems Al–Re, Nb–Os, Tc–Zr. Chi phases are assumed to be “electron compounds” (see Hume-Rothery phases). A number of chi phases transform to the superconducting state, with the highest transition temperature Tc = 12.9 K for Nb0.24 Tc0.76 (see Superconducting intermetallic compounds). CHIRALITY (fr. Gr. χειρ , hand)

Handedness, or belonging to one of two (“lefthand” or “right-hand”) non-superimposable mirror image conﬁgurations. See also Enantiomorphism. CHIRALITY IN LIQUID CRYSTALS

Absence of planes of symmetry in the molecules of liquid crystals. Chirality in liquid crystals leads to instability of a uniform (homogeneous) state, and the formation of spatially-periodic (spiral) structures (right-handed or left-handed) in some liquid crystal phases (cholesteric liquid crystals, blue phases, smectic liquid crystals of the C type); see Chirality, Enantiomorphism. CHIRALITY OF MAGNETIC BUBBLE DOMAINS The sign of the relative rotation of the magnetization in the center of a domain wall for a magnetic bubble domain with topological index S = 1, which does not contain Bloch lines. The magnetization in a magnetic domain wall is ei-

ther aligned along the vector tangent to the lateral surface of a domain wall, or is opposed to it. Hence two possible states of a magnetic bubble domain, labeled χ ± , are more favorable (in the context of magnetostatics) than all other states. By convention the label χ + is assigned to a clockwise rotation of the magnetization when observing along the rotation axis direction. The twisting deﬂections of χ + and χ − are equal in magnitude.

176

CHOLESTERIC LIQUID CRYSTAL

It should be noted that, by virtue of domain wall twisting, the above deﬁnition is valid only for the cross-section of the magnetic bubble domain by a plane that is at equal distances from the magnetic lm surfaces. Transitions between the χ + and χ − states of magnetization rotation usually occur when horizontal Bloch lines are present. CHOLESTERIC LIQUID CRYSTAL, cholesteric, chiral nematic, cholesteric phase (fr. Gr. χoλη , bile, σ τ ερεoς , solid, and χειρ , hand) An analog of a nematic phase (see Nematic liquid crystal) for a material containing chiral mole-

cules, that is molecules which differ from their mirror image structures (see Chirality in liquid crystals). When chiral molecules are dissolved in a nematic liquid the structure undergoes a helical distortion to form a helical phase called a cholesteric. This phase was originally observed in the ethers of cholesterol, hence its name. A cholesteric, like a nematic, lacks long-range order, and the molecular orientation has a preferred axis denoted by a director n which is perpendicular to the helical z axis. The local symmetry is close to ∞22 (or C∞h ), with the spatial distribution of the apex positions of the director vector n tracing out a spiral or helix. The spatial period or step along the helical axis is one half the pitch of the spiral because director orientations n and −n are equivalent, as is the case in nematics. The step of the spiral L depends on the chemical composition and on the temperature, and typical values lie in the range from 350 nm to 650 nm, corresponding to visible and near UV wavelengths. Cholesteric liquid crystals possess unique optical properties such as Bragg diffraction of light beams at the spiral structure, enhanced optical activity, etc. These properties are widely used in various ﬁelds of engineering, in particular in the medical area. CHRISTOFFEL SYMBOLS (E.B. Christoffel, 1869)

The Christoffel symbol is Γkli = g in Γn,kl , where the metric tensor gik deﬁnes Γi,k,l = (∂k gil + ∂l gki − ∂i gkl )/2, and ∂i = ∂/∂x i . The Christoffel symbols do not form a tensor; in particular by choosing a particular system of coordinates one may reduce all the Christoffel symbols to zero at any given point. In curvilinear coordinates in a

ﬂat space the Christoffel symbols are used to form covariant derivatives of tensors. These symbols are used in elasticity theory to characterize changes of the basis vectors ei of the local coordinate system deformed together with the body: dei = Γkil el dx k . Christoffel symbols and gik are both expressed through the strain tensor uik : gik = δik + 2uik (δik is the unit tensor), Γi,kl = ∂k uil + ∂l uki − ∂i ukl . To take into account dislocations and internal stresses, the Christoffel symbols are replaced, within the framework of the mechanics of solids, by the coefﬁcients of linear (afﬁnity) coherence, Γikl . The number of independent values of Γikl is equal to 15 (in contrast to 9 for the previous case). Γikl may be separated into symmetric (Γi(kl) ) and antisymmetric (Γi[kl] ) parts with respect to the indices k, l: Γikl = Γi(kl) + Γi[kl] . The quantity Γi(kl) characterizes the pure deformation of the trihedron deﬁned by the basis vectors ei , and Γi[kl] characterizes the rotation of the trihedron during its transition from point to point. The quantity Γi[kl] is directly linked to the density of dislocations in the material; the sum of the Burgers vectors of dislocations passing through a small area S is proportional to the convolution of the tensor of the area S and Γi[kl] . CHROME PLATING

Application of chromium coatings to the surface of materials to increase their hardness, wear resistance (see Wear), corrosion resistance and friction resistance, and also for decorative purposes. The thickness of the coatings varies from 1 μm to 3 mm, their hardness ranges from 500 to 1200 kg/mm2 . Electrolytic chrome plating is carried out from aqueous chromium-oxide solutions either with a sublayer of copper and nickel, or without it. The appearance, structure, physicochemical and mechanical properties of the coatings may be changed by variation of the electrolyte composition, and the method of electrolysis. Also in some areas of engineering diffusion chrome plating is used, preferably from the lowest halide compounds of chromium, by means of thermal decomposition or reduction in a gaseous, solid or liquid medium, with successive diffusion of chromium into the depth of the parts being coated.

CINNABAR

CHROMIUM, Cr

A chemical element of Group VI of the periodic table with atomic number 24 and atomic mass 51.996. There are four stable isotopes: 50 Cr, 52 Cr, 53 Cr, 54 Cr. The outer shell electronic conﬁguration is 3d 5 4s 1 . Successive ionization energies are 6.764, 16.49, 31, 51, 73, 90.6 eV. Atomic radius is 0.125 nm; radius of Cr2+ ion is 0.084 nm, of Cr3+ is 0.063 nm. Covalent radius is 0.118 nm. Oxidation states are +2, +3, +6. Electronegativity is 1.55. Under normal conditions chromium is a silvery-white metal. The crystal lattice is body¯ (O 9 ), with centered cubic, space group I m3m h parameter a = 0.28848 nm (at 298 K). Density 3 is 7.194 g/cm (at 298 K); Tmelting = 2176 K, Tboiling = 2742 K. Heat of melting is ≈14.0 kJ/mole, heat of evaporation is 393.34 kJ/mole; speciﬁc heat is 460 J·kg−1 ·K−1 (at 298 K). Debye temperature is 630 K. Linear thermal expansion coefﬁcient is ≈6.5·10−6 K−1 (at 298 K); coefﬁcient of thermal conductivity is 67 W·m−1 ·K−1 (at 298 K). Adiabatic elastic moduli c11 = 350.0, c12 = 67.8, c44 = 100.8 (in GPa). Young’s modulus is 279.65 GPa (at 298 K); shear modulus is 102.02 GPa (at 298 K), Poisson ratio is 0.31. Ultimate strength is 84 MPa (at 298 K, after recrystallization). Relative elongation is 0% (at 298 K, after recrystallization). Vickers hardness is 100 to 200 HV. Linear lowtemperature electronic speciﬁc heat coefﬁcient is 1.4 mJ·mole−1 ·K−2 . Electrical resistivity is 129 n·m. Temperature coefﬁcient of electrical resistance is 3·10−3 K−1 (293 to 373 K). Hall constant is 3.63·10−10 m3 /C (at 293 K). Coefﬁcient of absolute thermal electromotive force is 16.2 μV/C. Chromium is an antiferromagnet with Néel temperature TN = 311 K. Molar magnetic susceptibility is 3.6·10−6 CGS units. Nuclear magnetic moment is 0.474 nuclear magnetons. Reﬂection coefﬁcient of 500 nm wavelength light is 67%. Electronic work function of polycrystal is 4.68 eV. Chromium is employed to give glass an emerald green color, and it ﬁnds wide use as a catalyst. CHROMIUM ALLOYS Chromium-based alloys. Doping Cr with small additions (up to 1%) of yttrium, rare-earth elements and titanium causes the binding of these

177

atoms into refractory compounds (see Refractory materials), and reﬁning the metal matrix decreases the cold brittleness temperature slightly, and increases its plasticity. At the same time the corrosion resistance increases. Strong doping of Cr with iron, cobalt, nickel, ruthenium, and rhenium changes the electronic structure of chromium, and in some cases its crystal structure and phase composition. It provides for an appreciable decrease of the cold brittleness temperature. However, in such a case alloy brittleness appears, due to the formation of a sigma phase. Chromium alloys are smelted in archer or induction furnaces in an inert gas atmosphere, or fabricated by the method of powder metallurgy. A thermomechanical treatment of low-doped chromium alloys, when a ﬁnegrained and cellular dislocation structure arises (see Cellular structure), permits an increase of the strength and, at the same time, the cold brittleness temperature. Low-doped chromium alloys are used as thermal-environment resistant materials, and as high-temperature materials at 1000–1100 ◦ C, with a short-term heating capability up to 1500–1600 ◦ C. Highly-doped alloys are used in the chemical engineering industry, in the production of components for magnetohydrodynamic generators, foundry castings, etc. CINNABAR (fr. Gr. κινναβαρι), HgS A mineral, the red-colored stable modiﬁcation of mercury sulﬁde. The Mohs hardness is

2–2.5, and the density is 8.0–8.2 g/cm3 ; the crystal family is trigonal, and the space group is P 31 21 (D34 ), a = 0.4146 nm, c = 0.9497 nm. Another modiﬁcation of mercury sulﬁde, black metacinnabarite with the ZnS type structure, is unstable and gradually transforms into cinnabar. This most important mercury mineral is used to produce the metal. Artiﬁcially, cinnabar is prepared by rubbing mercury with sulfur with subsequent treatment with alkalis. The heat of formation equals −59 kJ/mol (at T = 298 K). Cinnabar exhibits a high volatility (t sublimation = 580 ◦ C). The crystal lattice energy is 3,578 kJ/mol. The crystals are composed of polymer chains –Hg–S–Hg–S– with the parameters: d(HgS) = 0.236 nm, ∠HgSHg = 105◦ , ∠SHgS = 172◦ . Artiﬁcial cinnabar is a semiconductor material used for photoresistors, as a catalyst, and as a pigment.

178

CIRCULAR PHOTOVOLTAIC EFFECT

CIRCULAR PHOTOVOLTAIC EFFECT Photovoltaic effect observed in doubly refracting crystals (see Gyrotropic media) illuminated by circularly or elliptically polarized light (see Polarization of light). There is a difference between

the circular photovoltaic effect and other photovoltaic effects: the resulting current is proportional to the degree of circular polarization of the radiation Pcirc and changes its direction in accordance with the sign of the polarization. The “circular” photovoltaic effect for elliptically polarized light is described by the following relation: jα = γαβ i[E × E ∗ ]β , where j is the current density, and E is the amplitude of the light electric ﬁeld (see also Bulk photovoltaic effect). For circular polarization this becomes i[E × E ∗ ] = |E|2 Pcirc q/q, where q is the wave vector of the light. Initially the circular photovoltaic effect was observed in tellurium, then it was studied in a variety of crystals including a number of ferroelectrics. The origin of this effect arises from the asymmetry of the distribution of the electrons excited by the light. This asymmetry is due to the correlation between the electron angular momentum (spin) and its linear momentum in gyrotropic crystals. The inverse effect, the so-called optical activity (see Rotation of light polarization plane) induced by the current and resulting from the spin orientation during the current ﬂow, has also been observed in tellurium. In nongyrotropic crystals, which possess no center of symmetry, the circular photovoltaic effect does not occur, while the phenomenon of optical activity may appear from uniaxial deformation or an applied magnetic ﬁeld. Such a magneto-induced circular galvanomagnetic effect was observed in p-type GaAs. In crystals of low symmetry, including those possessing a center of symmetry, the circular drag effect described by the relation jα = Tαβγ i[E × E ∗ ]β qγ may be observed. In contrast to the circular photovoltaic effect, the circular drag effect is due to the transfer of phonon momentum to the electrons. The current in this effect changes its sign, not only when the

sign of the circular polarization changes, but also when the light propagation direction changes. The circular photovoltaic effect may used in inertialess receivers of polarized laser radiation, in elements of optical memory on photorefractive crystals (see Photorefraction), and also as a mechanism of fourwave mixing of isofrequency waves in various nonlinear optical frequency converters. CLATHRATE COMPOUNDS (fr. Gr. κληθρα , adler-tree) Phases comprising at least two compounds,

with the molecules of one enclosed in the molecular voids or lattice cavities of the other. They bear a close similarity to interstitial solid solutions. As a rule, only van der Waals forces act between the molecules of a clathrate compound. The binding energy of each enclosed molecule is about ≈50 kJ/mol. This relatively high value for van der Waals interaction is explained by the molecule and void geometry ﬁtting well into one another, and by the many points of bonding by the molecule. Depending on the void type, clathrate compounds are categorized as lattice or molecular types. Lattice clathrate compounds can only be solids, and are further classiﬁed by the shape of their voids as channel, cage (originally only this type was termed clathrate), and laminated varieties. Examples of “host” compounds that form cage clathrates are uria, thiouria, hydroquinone, phtalocyanines, etc. There is a wide range of corresponding “guest” compounds: hydrocarbons, alcohols, many gases. Cyclic molecules usually form the molecular clathrate compounds, such as cyclodextrin and other macrocyclic compounds. Compounds of relatively small dimensions can be enclosed in the voids of such “hosts”. The clathrate compounds exhibit, in the general case, a variable composition. They are employed mainly to isolate and purify “guest” molecules. CLAUSIUS–MOSSOTTI EQUATION (R. Clausius, O. Mossotti, 1879)

Relation between the relative (dimensionless) dielectric constant of isotropic nonpolar insulators, ε(ω), at a frequency ω (see Temporal dielectric dispersion) and the polarizability, α(ω), of the atoms that make up the crystal lattice:

α(ω)N ε(ω) − 1 = , 3ε0 ε(ω) + 2

(1)

CLOSE-PACKED STRUCTURES

where N is the number of atoms per unit volume, and SI units are used. This expression is sometimes written in terms of the electric susceptibility χ(ω) = ε(ω) − 1. If the square of the refractive index, n(ω), in the transparency region is substituted for ε(ω) then Eq. (1) is called the Lorentz–Lorenz relation. Eq. (1) differs from the frequently used expression ε = 1 + αN/ε0 which is applicable in the case of a linear response of a medium (crystal) to a macroscopic electric ﬁeld averaged over the medium, since the Clausius–Mossotti equation is derived taking into account the local electric ﬁeld that acts on an atom in the crystal, and this differs from its mean value. The Clausius–Mossotti equation for cubic crystals coincides with the expression for ε derived from the rigorous Ewald method. See also Langevin–Debye equation.

179

Fig. 1. Planar triangular close packing arrangement of spheres.

CLEMENTI FUNCTION (E. Clementi)

A wave function of a certain nl-shell of an atom (or ion) whose radial part is represented as a superposition of Slater functions (see Slater rules), the parameters of the latter being derived from minimizing the total energy of a given multielectron state. Clementi functions can be used as the ﬁrst approximation for a non-empirical computation of crystals. CLOSE-PACKED STRUCTURES, closest-packed structures

Geometrical arrangement of rigid spheres of the same radius, which provides the densest ﬁlling of space. There is only one way of attaining such a conﬁguration in a plane, which consists in arranging a lattice (the sites formed by the centers of balls) based on an equilateral triangle conﬁguration, as shown in Fig. 1. The threedimensional closest-packed sphere structure is constructed from the above planar arrangement by superimposing layers, one onto another, in such a way that the upper layer of a pair lies with its atoms set in the recesses of the layer below; the density of√packing (packing fraction) in this case being π/ 18 ≈ 0.74. There are two ways to do this, and either one is effectively equivalent. The third layer also has two possibilities, but they are not equivalent. One way for positioning the third layer is to place its spheres in recesses between second layer atoms that are not directly above the

Fig. 2. Three-dimensional close packing arrangements of spheres: (a) face-centered cubic, and (b) hexagonal close-packed.

atoms of the ﬁrst layer, and this gives what is called an ABC arrangement of layers, as shown in Fig. 2(a). None of the three layers is directly above another. Another way to position the third layer is with its atoms in recesses directly above the ﬁrst layer, thereby forming what is called the ABA sequence of layers, as shown in Fig. 2(b). Each subsequent layer can be positioned in one of two ways, leading to an inﬁnity of possible closest packed structures if the number of layers becomes very large, and the sequencing of the A, B, and C type layers is random subject to the condition that two identical layers cannot be adjacent to each other. If the sequence is a periodic one, then the corresponding closest-packed sphere structure is spoken of as periodic highest-density spherical packing. According to the Belov theorem, periodic closest-packed sphere structures may exhibit only eight different space groups of symmetry: P 3m1, R3m, P 3m1, R3m, P 6m2, P 63 mc, P 63 /mmc, F m3m. The packing consisting of only two alternating layers ABAB. . . is referred to as highest-

180

CLOSE PACKING, RANDOM

density hexagonal packing or hexagonal closepacked (HCP). The three-layered ABCABC. . . arrangement is given the name highest-density cubic packing or cubic close packing (CCP or FCC). The centers of the spheres of the latter structure form a face-centered cubic lattice. The tendency of atoms to attain closest packing results in the fact that most metallic atoms crystallize in one of the close-packed arrays which is almost always the hexagonal (e.g., Mg, Nd, Zn) or the facecentered cubic (e.g., Ag, Al, Cu) one. In addition bulky components (e.g., anions oxygen or sulfur) of various widely occurring chemical compounds also form close-packed arrays, and the diversity of structures stems from the fact that there are many ways of arranging the smaller cations throughout the smaller tetrahedral and larger octahedral cavities of the closest-packed structure. CLOSE PACKING, RANDOM See Random close-packing model. CLUSTER

A stable aggregation or group of atoms or molecules distinguished by certain physical or chemical features from other similar stable microobjects. Several particles constitute the lower limit on the size of a cluster, while the upper limit can often be deduced from one of the following two traits: (1) the addition of one more particle to the aggregation appreciably affects the system properties; or, (2) the number of particles at the surface, i.e. those which differ in properties from the bulk due to their proximity to the surface, is comparable to the total number of internal particles in the cluster. These conditions usually limit the number of particles in a cluster to the range 102 –103 . Larger agglomerates of particles in a material are called phase precipitates. Examples of clusters are: agglomerations of impurity atoms or intrinsic defects (see pile-up of dislocations and point defect clustering) arising in the bulk of a solid due to their mutual attraction and to the diffusion of particles (during the growth of crystals or during heat treatment), under the action of external energetic particles (see Collision cascade and Subcascades), under the action of light (in photographic emulsions), etc. The atomic or molecular

aggregates that comprise a small particle can be formed during the coagulation of particles, e.g., those dispersed in air (aerosol particles), during the sputtering of materials under ion bombardment or other high-energy factors, during evaporation, etc. Surface clusters can be formed by deposition of particles on the surface of a solid. The stability of a cluster can depend on the number n of constituent particles, and sometimes it depends on whether n is odd or even. Thus it was established by means of mass spectrometry that when Li atoms are evaporated into an inert gas an appreciable amount of Li2 , Li6 and Li8 appears, whereas Li3 , Li5 , Li7 , and Li9 are either entirely absent, or are present in only trace amounts. During the ion sputtering of Ag crystals three times more Agn clusters form with odd n compared to the number with even n. A method termed the cluster approximation is often employed in numerical computations of the energy spectra of ideal crystals, or of crystals with defects, with a cluster deﬁned here as a lattice of a ﬁnite number of atoms. Atom–atom potentials and cluster boundary conditions are chosen to provide for a high cluster symmetry, for correct values of the crystal lattice constants, and for stability. Systems of particles can also have fractal properties (see Fractal) arising from special rules followed in building the system. For instance, a percolation cluster is a set of certain lattice sites obtained by successive translations of a given length from an arbitrarily chosen starting site to other randomly chosen sites; the dimensions of such a cluster are not limited to integers (see Percolation theory). In quantum scattering theory coupled states of several particles are termed clusters; with every cluster considered as a separate scattering channel. CLUSTER APPROXIMATION

The breaking down of a system into subsystems (see Cluster) that interact weakly with each other. This approximation is employed in thermodynamics, statistical physics, and quantum scattering theory. It involves expressing the wave function of a multiparticle system far away from the scattering region as a superposition of states corresponding to individual isolated particles and/or groups of them. The cluster approximation in the

COADSORPTION

theory of lattice defects in crystals is based on singling out a region in the crystal that incorporates the defect and several coordination spheres surrounding it. The local defect properties (binding energy, energy level position, wave function of the localized state, lattice conﬁguration) are then computed over this region using one of the standard molecular theory methods. The interaction of the cluster with the rest of the crystal is accounted for by using a self-consistent eld approach. Sometimes the term cluster approximation is employed to designate an approximate method for computing the parameters of an ideal crystal by representing the crystal as a cluster consisting of a relatively small number of atoms. Certain boundary conditions are imposed upon the outermost atoms to ensure the stability of such a conﬁguration. See also Watson sphere. CLUSTER, CYBOTAXIC See Cybotaxic clusters. CLUSTER DEPOSITION

Formation of heterogeneous lm s composed of clusters of particles. The ﬁlms form via the deposition from a ﬂow of clusters, e.g., produced by ion sputtering of different targets, or by homogeneous gas phase nucleation, or due to a heterogeneous nucleation at the substrate surface. A cluster may contain from several to a few thousand particles. An assortment of cluster deposition technology methods provides a range of structures and cluster properties which determine the ﬁlm formation kinetics and ﬁlm properties. Using the method of cluster deposition at low temperature one can obtain the epitaxial deposition of multicomponent compounds such as semiconductors, or one can grow diamond-like carbon lms, oxides, nitrides, carbides, etc. CLUSTER, NONCRYSTALLINE See Noncrystalline clusters. CLUSTER SPUTTERING Sputtering of a solid under the action of ion bombardment during conditions when clusters of

different size composed of the solid’s own atoms plus impurity atoms are predominant in the ﬂux or ﬂow of sputtered material. Not only neutral

181

clusters, but also positive and negative ions, polyatomic and molecular ions and their fragments, are found in the sputtered ﬂux during the cluster sputtering of metals, semiconductors, insulators, organic compounds, polymers and biomolecules. The mass-spectra of sputtered clusters range from dimers through aggregates of tens and hundreds of atoms, up to large bioorganic molecules and their clusters. The energy distribution of sputtered clusters reaches 100–200 eV, the average being 2–10 eV per cluster of ions and 10–20 eV for neutral clusters. The sputtering probability sharply drops with an increase in the number of atoms in the cluster, and it can undergo oscillations associated with the binding energy. In particular, there may be less charged metallic clusters having an even number of atoms than those having an odd one. The mechanisms of the cluster sputtering of solids are not yet understood. Theories of direct knock-out (for small clusters), of recombination, and of shock waves, have been proposed to explain the phenomenon. The latter theory allows for the emergence of large clusters and of complete bioorganic molecules (such as insulin) under the impact of a single heavy accelerated ion, or of a fragment from nuclear ﬁssion. Cluster sputtering plays an important role in secondary ion mass-spectrometry, and it also ﬁnds applications in designing sources for accelerated cluster and macromolecular ion formation, including ionized bioorganic molecules. COADSORPTION

A cooperative adsorption of adsorbates of differing chemical composition. In the case of physisorption the mutual inﬂuence of these adsorbates is associated with the difference in the heats of adsorption, which may result in the particles with a greater heat of adsorption driving out those with lesser heats of adsorption. In the case of chemisorption, the mutual effects of the adsorption of different species is associated with the formation of chemical bonds of the adsorbates with the substrate; this can result in a promotion or inhibition of the sorptional activities of neighboring centers. Such an inﬂuence may stretch over the distance of several lattice constants, and may result in the emergence of not only a short-range, but also a long-range order. The phenomenon of

182

COAGULATION

heterogeneous catalysis is based on the process of coadsorption of molecules of differing chemical composition.

COAGULATION

See Coalescence.

COAL

Carbonaceous porous combustible stratiﬁed rock; with a surface of fracture which is either lustrous or lusterless. Coal contains a maximum of 30% of incombustible components (ash). Coal is formed by carbonization (metamorphic transformation) of the remains of decomposed plants under prolonged exposure to temperature, ionizing radiation of natural radionuclides, etc. According to the degree of carbonization, brown coal (lignite) and black coal are distinguished. The carbon content increases from ∼65% (by mass of organic components of coal) for soft lignites to >91% for anthracites; accordingly, the oxygen content decreases from 30 to 2%, and the hydrogen content decreases from 8 to 91% C exhibit an abrupt increase of aromaticity, and an abrupt decrease of electric resistance. Coals contain paramagnetic centers, with concentration reaching 1020 spin/g.

COALESCENCE (fr. Lat. coalesco, grow together, be coupled) The spontaneous merger of small particles of

a solid that results in the formation of a single larger particle whose shape minimizes its free energy. The phenomenon of the formation of pores in a solid is also known. The coalescence of particles may occur in sols, aerosols, and on the surface of a solid. Coalescence is distinct from coagulation, the latter being the mere sticking together of colliding particles. Coalescence is associated with diffusion processes that take place under the inﬂuence of surface tension forces. It will be slowed down by charged particles. Surface coalescence is conditioned by strains in the substrate, by its surface roughness, and by its polycrystalline structure. COATING

Application of a layer, which has protecting, decorating, conducting, etc., properties, to the surface of a material. Metals and alloys, as well as nonmetallic substances, are used as coating materials. Application of a metallic coat is performed through hard facing with a thin layer of salts in oil (baking coating), chemical deposition, galvanization (electrolytic deposition, see Electroplating), dip coating (dipping into melted metal or into aqueous salt solutions in the presence of oxygen), vacuum evaporation, cathode sputtering (sprayed metal coating), etc. Nonmetallic coats (varnishes, enamel and oil paints) are applied to surfaces through brushing, spraying under pressure, fusion. Colloid mixtures of graphite with varnish, or of a metal with varnish, are used as nonmetallic conducting coatings. Anodic oxidation is used in order to coat the surface with an oxide lm ; carbon ﬁlms are obtained through decomposition of a dried layer of carbonic acid through heating to 473 K, or high vacuum evaporation. COATING, ANTICORROSIVE See Anticorrosive coatings. COBALT (Lat. cobaltum ), Co

Chemical element of Group VIII of the periodic system with atomic number 27 and atomic mass 58.9332. The naturally occurring stable isotope 59 Co is very close to 100% abundant. The

COERCIVE FORCE

most important artiﬁcial isotope is radioactive 60 Co with a half-life of 5.24 years. The outer shell electronic conﬁguration is 3d 7 4s 2 . Successive ionization energies are 7.865, 17.06, and 33.50 eV; electronegativity is 1.7. Atomic radius equals 0.125 nm; the Co2+ ionic radius equals 0.072 nm, that of Co3+ is 0.063 nm. The oxidation state is +2, +3, rarely, +1 and +4. Cobalt in the free state is a metal of silver-steel color. It exists in two polymorphic conﬁgurations: α-Co with a hexagonal close-packed lattice (space 4 ), a = 0.2507 nm and c = group P 63 /mmc (D6h 0.40686 nm at 298 K), and β-Co with a facecentered cubic lattice (space group F m3m (Oh5 ), a = 0.3548 nm). The temperature of the start of the transformation of α-Co into β-Co by heating is 750 K; the temperature of the start of the reverse transformation by cooling is 676 K. The density of α-Co is 8,183.6 g/cm3 (at 293 K), that of β-Co is 8,739 g/cm3 (at 298 K), the binding energy is −4.387 eV/atom at 0 K and −4.4 eV/atom at room temperature; T melting = 1768 K, T boiling = 3203 K. The heat of fusion is 16.2 kJ/mol. The speciﬁc heat is 414 J·kg−1 ·K−1 at standard pressure and temperature. The Debye temperature is 385 K. The coefﬁcient of linear thermal expansion parallel to the c axis is 14.62·10−6 K−1 , and perpendicular to the c axis, it is 10.96·10−6 K−1 . The thermal conductivity is 142 W·m−1 ·K−1 at 163 K and 70.9 W·m−1 ·K−1 at 290 K; the adiabatic elastic rigidity coefﬁcients of α-Co crystal are: c11 = 306.28, c12 = 165.12, c13 = 101.9, c44 = 75.33, and c33 = 357.4 GPa at 298 K. Young’s modulus of α-Co is 220.9 GPa, that of β-Co is 199.7 GPa; the modulus of rigidity of α-Co is 84.5 GPa, that of β-Co is 74.7 GPa; Poisson ratio of α-Co is 0.307, and that of β-Co is 0.337 (at 298 K). The ultimate tensile strength is 260 MPa (at 298 K), and the relative extension is 5% (at 293 K). The Brinell hardness is 124 MPa for cobalt subjected to 1.2–3 GPa treatment. The self-diffusion coefﬁcient equals 5.91·10−26 m2 /s. The Sommerfeld low-temperature electronic speciﬁc heat coefﬁcient (linear term) equals 4.73 mJ·mol−1 ·K−2 . Electrical conductivity is 55.7 n·m (at 293 K); the temperature coefﬁcient of electric resistance equals 604·10−5 K−1 . The Hall coefﬁcient is

183

0.36·109 m3 /C. The absolute thermal electromotive force coefﬁcient equals 18.5·10−6 V/K. The optical reﬂectivity for 5.0 μm wavelength is 92.9%. The work function for a polycrystal equals 4.41 eV. Cobalt is a ferromagnet with Curie point T C = 1393 K. The nuclear magnetic moment of 59 Co equals 4.639 nuclear magnetons, and the atomic magnetic moment equals 1.715 Bohr magnetons. The thermal neutron absorption crosssection is 34.8 barn. Cobalt ﬁnds its use as a component of hard magnetic, corrosion resistant and high-temperature alloys and coatings, as well for glass dyeing; the intermetallic compound SmCo5 is used for the fabrication of permanent magnets (see Samarium– cobalt magnet), and radioactive 60 Co is employed in medicine as a source of γ -radiation. COERCITIMETER

Device for measuring the coercive force or coercivity Bc of magnetic materials. The most common types are coercitimeters for coercive force measurement by magnetization MBc or by induction BBc . For an MBc measurement the sample is magnetized to saturation and then demagnetized up to the point of zero magnetization, and the magnetic ﬁeld strength that brings this about corresponds to MBc . For measuring Bc by induction the sample is made part of a closed magnetic circuit, and the strength of the demagnetization ﬁeld at which the induction B in the sample goes to zero is accepted as the value Bc (i.e., BBc ). For small values of the coercive force MBc ≈ BBc . See Magnetometry, Magnetic structure analysis. COERCIVE FORCE, coercive e ld, coercivity (fr. Lat. coercitio, con nement)

Value of an applied magnetic ﬁeld Bc which reduces the magnetization of a magnetized magnetic substance to zero. In many magnetic materials the magnetization process is not reversible, but takes place around a hysteresis loop. An applied magnetic ﬁeld Bm produces a state of magnetization Mm in the material. The removal of the applied ﬁeld does not reduce the magnetization to zero, but rather to the remanent magnetization value Mrem . A reverse direction ﬁeld −Bc must be applied to reduce the magnetization to zero. Increasing the reversed applied ﬁeld to −Bm induces the reversed magnetization −Mm , and most

184

COHERENCE

of a hysteresis loop is thereby traced out. When Bm is small the coercive ﬁeld Bc is also small, where of course Bc < Bm , and increases in Bm cause Bc to increase. Very large applied ﬁelds Bm induce a saturation magnetization Ms , so further increases in Bm have no effect. The coercive ﬁeld Bc measured at saturation is called the coercivity, and the associated hysteresis loop is called an extremal hysteresis loop. The coercivity of various materials varies over a very wide range from 10−4 mT to 10 T. (Some authors deﬁne Hc = Bc /μ0 , where 1 mT ∼ = 795.8 A/m.) The coercivity arises from the back magnetization process, and involves the magnetic anisotropy energy, the magnetostriction, and the saturation magnetization. In a particular material the coercivity can differ considerably depending on its structural state; it depends also on the direction in anisotropic materials, on the temperature, and on the presence of external stresses. The extremal coercivity value for a given material equals its anisotropy ﬁeld and can be achieved, e.g., in ﬁne monocrystal ferromagnetic single-domain particles, in which back magnetization is brought about by irreversible rotation of the spontaneous magnetization vector. High coercivity values can be obtained in close to perfect crystals where, near saturation, the formation and growth of back magnetization nuclei are impeded. In most ferromagnets the coercivity is determined by the critical ﬁeld for irreversible displacement of magnetic domain walls, and this can be impeded by various inhomogeneities such as internal stress gradients, foreign inclusions, structural defects, and so on. COHERENCE See Macroscopic quantum coherence, Structural coherence. COHERENCE FACTORS

Renormalization coefﬁcients F 1,2 (k, k ) appearing in the Bardeen–Cooper–Schrieffer theory (BCS theory) which connect the matrix elements B1 (k , s | k, s) for single-particle transitions k, s → k , s in the system of non-interacting Bogolyubov quasi-particles (see Bogolyubov method), and the matrix elements B2 (k , s | −k, −s) for the processes of the annihilation of quasiparticle pairs in the states k , s and −k, −s. The

latter appear in a superconductor under the effect of an external perturbation with corresponding matrix elements B0 (k , s | k, s) for the singleelectron transitions k, s → k , s in the normal state of a metal: B1,2 = F1,2 B0 . According to the BCS theory, F1 (k, k ) = Uk Uk ± Vk Vk , F2 (k, k ) = Uk Vk ± Uk Vk , where the Uk , Vk are the Bogolyubov transformation coefﬁcients (see Canonical transformation method), with the sign determined by the nature of the external perturbation. Coherence factors are needed for theoretical descriptions of the different kinetics in superconductors associated with transitions in the system of Bogolyubov quasi-particles. This provides, e.g., in the BCS theory, an explanation of the difference between the type of temperature dependence of the nuclear spin relaxation time and that of the coefﬁcient of ultrasound adsorption in a superconductor. COHERENCE LENGTH in superconductors

Length scale for the variation of the order parameter (see Ginzburg–Landau theory of superconductivity) ξ0 , ξ(T ) = √ 2(1 − T /Tc )1/2

ξ0 =

vF , πΔ0

where v F is the Fermi velocity, Δ0 = E g /2 is the superconducting energy gap at T = 0, and T c is the critical temperature of the second-order phase transition from the normal to the superconducting state. According to the scale invariance hypothesis, at the point T = T c the coherence length ξ goes to inﬁnity as ξ(T ) ∼ (1 − T /T c )−ν . The critical index is ν = 1/2 in the self-consistent e ld approximation. The coherence length also determines the effective size of Cooper pairs with the binding energy 2Δ. In pure superconductors with T c ≈ 1–10 K, for T T c , ξ is equal to ξ0 ≈ 10−5 –10−4 cm in order of magnitude. In “dirty” superconductors with short electron mean free paths l ξ(T ) the effective coherence length is ξ eff ∼ = (ξ l)1/2 . In highly disordered superconducting alloys (compounds) and in amorphous superconductors ξ 10−6 cm, which provides

COHERENT BREMSSTRAHLUNG

185

high values of the Ginzburg–Landau parameter κ = λ/ξ and the upper critical eld B c2 (T ), where λ is the magnetic ﬁeld penetration depth. COHERENT BREMSSTRAHLUNG A type of Bremsstrahlung (braking radiation) speciﬁc for monocrystals. The Bremsstrahlung of

charged particles in single crystals at high particle energies effectively differs from that of an isolated atom. For relativistic particles (total energy E far exceeds rest energy, Lorentz factor γ = [1 − (v/c)2 ]−1/2 E/(m0 c2 ) 1), there is a formation zone one radiation length l long in which the Bremsstrahlung process takes place which can substantially exceed an atomic size, i.e. the creation of a radiated photon takes a long enough a time so that a particle can traverse a macroscopic distance. The time of photon generation is long compared with the duration of a particle’s impact upon a nucleus, therefore the process characteristics are determined mainly by interference during the radiation process, rather than by the nature of the collision with an individual nucleus. The formation zone in monocrystals may be substantially longer than the separations between the atoms of the crystal lattice. In this case all the atoms in the zone take part in the process of coherent radiation, with the Bremsstrahlung intensity in monocrystal increasing, relative to that of an an amorphous substance, proportional to the number of atoms located in this zone: N eff ∝

l 2E(E − ω) ∝ . a m2 c3 ωa

The presence of interference in the monocrystal Bremsstrahlung arises from simple kinematic considerations. Suppose a particle entering a crystal at a small angle, θ , relative to a crystallographic axis encounters atoms along its path spaced a distance a/θ apart (a is the lattice constant), and subsequent acts of Bremsstrahlung emission take place. Suppose the energy of the radiation of quanta is small, and the radiation only weakly affects the particle motion (its momentum is virtually unchanged at radiation). The quanta are emitted mainly in the forward direction of the particle motion (within a cone whose angle is inversely proportional to the Lorentz factor γ ). If t0 is the time of emission at the ﬁrst atom, the

Intensity I of Bremsstrahlung of electrons in a diamond single crystal as a function of the energy ω of the emitted quanta at the incidence angle θ = 4.6 mrad relative to the (110) axis (an electron beam of initial energy 1 GeV is directed along the (001) plane); shown are theoretical calculations (solid lines) and experimental data (dots).

Bremsstrahlung emission at the second atom will occur at the time t0 + a/(vθ). As the ﬁrst emitted quantum reaches the second atom at the moment t0 + a/(cθ), the phase difference between the two must be equal to 2πn (where n is an integer) for the interference to amplify the radiation: a 1 1 = 2πn. − ω θ v c With a ﬁxed particle energy, E, and a ﬁxed magnitude of quantum energy, ω, there is a particular angle θmax at which constructive interference is observed: a , θmax = 2πnl where l is the radiation length. There may be different numbers of lattice sites inside the Bremsstrahlung region, depending on the angle of incidence of the charged particle relative to the crystallographic planes or axes, which results in an appearance of maxima and minima in the Bremsstrahlung spectrum presented as a function of the angle at which fast particles enter the monocrystal. The intensity of coherent Bremsstrahlung in the Born approximation is proportional to the square of the number of atoms within the radiation length. If the Born approximation is inapplicable, the dependence of coherent emission intensity I on the number of atoms

186

COHERENT CHANNELING

within the formation zone is weaker, having a logarithmic dependence (see Fig.). The coherent Bremsstrahlung exhibits a rather high degree of polarization, and this results in intense beams of polarized γ -quanta being produced by electron accelerators. COHERENT CHANNELING See Okorokov effect. COHERENT CONDENSATE See Bose condensate. COHERENT POTENTIAL METHOD (P. Soven, D. Taylor, 1967)

An analogue of the mean ﬁeld method used for computing the electronic structure and electronic properties of disordered alloys (see Disordered solids) based on the formalism of multiple scattering theory. The applicability of this method is not related to limitations on the magnitude of the impurity scattering potential, or of the alloy component ratios. A scattering matrix (t -matrix) is assigned to each individual atom in this approach. Systems of atoms are described on the basis of the scattering characteristics of individual atoms using a Green’s function that depends upon the positions of the scattering atoms. It is assumed that the energy spectrum of the ensemble as a whole can be “macroscopically” described with the mean Green’s function −1 G(z) = z − ε(k) − (z) ,

k

where k (z) is a self-energy term (see Mass operator of quantum mechanics), and ε(k) is the dispersion law for an electron in an unperturbed translationally-invariant crystal. To complete the Green’s function deﬁnition, the system is presumed to behave as if one and the same coherent potential, σ (z), is assigned to each lattice site, and an effective potential, w n = wn − σ (E), is introduced for every site to replace the random potential energy of an electron wn (see Random potential). The self-consistency condition is taken as follows: w n = 0. tn = 1−w n n|G(z)|n

This implicit equation deﬁnes σ (E) ≡ k (E), and permits the determination of the coherent potential as a function of a spectral variable z. This method is believed to provide one of the best single-site approximations for obtaining the spectral characteristics of disordered systems. The small parameter of the method for the calculation of the energy spectrum is the quantity (a/R0 )3 , where a is a lattice constant, and R0 is a characteristic damping or jump length of the hopping integral. A similar small parameter appears when computing corrections to the expression for the electrical conductivity of a disordered binary alloy within the formalism of the coherent potential method. The physical sense of this parameter can be explained as follows: if a sphere of radius R0 encloses a large number of sites then one can neglect the ﬂuctuations of the number of atoms of both types A and B inside this sphere. COHERENT PRECIPITATES New phases formed at phase boundaries which display a structural coherence there. Coherent

precipitates arise as a result of the decomposition of supersaturated solid solutions (see Alloy decomposition), or from other phase transitions: a martensitic transformation, a eutectic (see Eutectic alloys), etc. Coherent precipitates may be wholly or partially coherent, depending on the type of structural coherence. They form during the early stages of phase transformations; later on, the structural coherence will be destroyed due to structural dislocations which form at the phase interface to make the precipitates non-coherent. The appearance of coherent precipitates with an appreciable mismatch of crystal lattice constants δ = (a p − a m )/a m , where a p and a m are lattice constants of the precipitate and matrix, respectively, gives rise to coherent elastic stresses, and to an increase of the elastic energy of the system by a magnitude εe ∝ δ 2 . That results in an increase of the strength of an alloy, of its coercive force, and of the magnetostatic energy (see Magnetostatics). In aging alloys (see Alloy aging), the elastic interaction of coherent precipitates may produce modulated structures. Coherence disruption, and an appearance of non-coherent precipitates, will usually result in deterioration of the alloy strength characteristics.

COLD BRITTLENESS

COHERENT SCATTERING REGIONS Largest regions of a crystal from which elastic scattering of radiation (X-rays, neutrons, etc.) by individual atoms or unit cells is coherent. The di-

mension D of a coherent scattering region can be deﬁned as the distance at which the phase shift of the waves scattered by atoms (cells) reaches π as compared to an ideal crystal. The value of D depends on the reﬂection indices hkl of the planes. In the case of an ideal mosaic crystal, D coincides with the size l of mosaic blocks. Provided the disorientation of adjacent blocks is ψ λ/ l (λ is the radiation wavelength), the value of D may be estimated from the width δθ of the X-ray line at its half-height: D ≈ λ/( θ · sin θ B ), where θ B is the Bragg angle. In the opposite case (when ψ λ/ l), the regions of coherent scattering may cover several blocks (D ∝ λ/ϕ > l). The blocks of the mosaics do not exclusively determine the range of coherent scattering in a real crystal. Stacking faults (leading to an effective reduction of the coherent scattering regions), small-angle boundaries, degree of uniform bending of crystallites, and internal microstresses in crystallites also play roles. To separate the effect of mosaics from that of microstresses, one may apply harmonic analysis to calculate the normalized Fourier coefﬁcients An in the reﬂection curve (the proﬁle of the X-ray line), P (2θ). The values of An can be written as the product An = An An , where An , An are the contributions from regions of coherent scattering and of microstresses, respectively. In the xyz coordinate system, with xy planes coinciding with reﬂecting planes, one may deﬁne the dependence of An on the reﬂection index 00l and then, extrapolating An (l) to l = 0, ﬁnd An = An (0). The derivatives of An characterize the average size D0 of the coherent scattering region, and the distribution Pn of the regions of coherent scattering transverse and along the z axis direction: −(dAn /dn)n=0 = c/D0 (c is the unit period along the z axis), d2 An /dn2 = Pn . COHESION (fr. Lat. cohaesus , stuck)

Linkage (binding) between two solid bodies of similar chemical composition in contact with each other. It results from a balance between longrange repulsive and short-range attractive forces. The cohesion energy is an important characteristic associated with chemical bonds. It is deﬁned as

187

the work required to move far apart the units of a bound structure. It can be experimentally found by evaporation or sublimation. The largest cohesion energy values are found in condensed phases (liquids and solids) where the chemical bonds are mainly ionic, covalent or metallic in character. The cohesion energy in real gases is several orders of magnitude smaller. The cohesion strength depends on the mutual orientations of the crystal lattices of the bodies in contact, on their geometrical perfection, and on the degree of their surface cleanliness. The cohesion strength is calculated from the expression P = (α10 + α20 − α12 )/a where α10 and α20 are the speciﬁc energies of the surfaces in contact, α12 is the speciﬁc energy of the grain boundary interface, and a is an interatomic distance. If the contacting surfaces are aligned relative to the symmetry elements then α10 = α20 = α, α12 = 0, and Pmax = 2α/a. The actual strength is smaller than Pmax due to the lack of smoothness of an actual contact. Showing up in the cohesion linkage zone are stresses arising from mismatches in the crystal geometry of the surfaces in contact. COINCIDENT-SITE LATTICE An auxiliary lattice considered in the description of particular grain boundaries. A coincident-

site lattice is that sublattice of the complete superposition lattice whose sites are occupied by atoms of both lattices of a bicrystal, i.e. the sites coincide in each of the crystals that are separated by the boundary. The reciprocal relative fraction of coincident sites is designated by Σ . The symmetry of the coincident-site lattice is determined by the symmetry of the pair of conjugated crystals, by the axis of their relative orientation, and by the value of the corresponding rotation angle. See Grain boundary, Grain boundary lattice. COLD BRITTLENESS

The change of the failure mechanism from tough failure to brittle failure (or quasi-brittle failure), which occurs with a decrease of temperature within a comparatively narrow temperature range. This change of failure mechanism involves abrupt reduction of plasticity-related characteristics and strength. According to the Ioffe theory, cold brittleness is the consequence of an abrupt increase of

188

COLD CATHODE

the yield limit σs with decreasing temperature, the temperature dependence of the breaking stress σf being comparatively weak. Cold brittleness occurs below the temperature at which the curves of σs (T ) and σf (T ) versus T intersect. Modern microscopic dislocation theories attribute the sharp temperature dependence of the yield point to the presence of a covalent component in the interatomic bond (see Covalent bond), and to the high value of the Peierls–Nabarro stress (see Peierls– Nabarro model) at the plastic deformation of covalent crystals. Hence the cold brittleness arises due to the abrupt decrease of the mobility of dislocations with decreased temperature, and to the decrease of the rate of stress relaxation at the apexes of cracks and at other stress concentrators (see Stress concentration). The reciprocal of cold brittleness is given the name cold reluctance. This term is descriptive of the ability of materials to retain plasticity and failure toughness with decreasing temperature. The susceptibility of a material to cold brittleness is determined by the cold brittleness temperature (or cold brittleness threshold) Tc . Upper u and T l ) and the lower cold brittleness points (Tcb cb l are commonly distinguished. The lower point Tcb is the minimal deformation temperature at which plastic deformation precedes the failure, and the failure is totally tough in its nature. The value of u depends heavily on the deformation rate ε˙ , Tcb increasing with its increase. Various methods of hardening of materials (raising the dislocation density): solid-solution hardening, dispersion hardening (see Precipitation-hardened materials), etc. l . Only a result in an increase of the value of Tcb reduction of the crystal grain size or the formation of a disoriented dislocation cellular structure can lead to the reduction of Tcb and the improvement of strength properties. As the failure mechanism changes from transcrystalline failure to intercrystalline failure, the cold brittleness temperature may abruptly increase.

ﬁlms, semiconductor ﬁlms, p–n junctions biased in the gate direction (see Semiconductor junction), transistor structures, M–I–S structures (see Metal–insulator–semiconductor structures), M–S structures (M is metal, I is insulator, S is semiconductor), semiconductor structures with a negative electron af nity, etc. COLD ELECTRONS

An electron gas in the conduction band of semiconductors (holes in the valence band) with an average energy ε appreciably less than the thermodynamic equilibrium value ε0 . This phenomenon of electron cooling is due to various mechanisms related to the motion of the current carriers in an electric ﬁeld, or to optical transitions of the charge carriers. For instance, electron cooling will occur if the overall current in a semiconductor is directed opposite to the internal electric ﬁeld in a space charge region, or because of another inhomogeneity of the semiconductor. In electric ﬁelds, where the current is directed along the ﬁeld, a cooling of the carriers is possible when the dominant scattering of the electron energy occurs by optical phonons, and the momentum scattering is by ionized impurities under conditions when the electron–electron interaction is negligible. While acted on by an electric ﬁeld an electron is able to emit an optical phonon, and thereby diminish its energy (i.e. cool), and the scattering by ionized impurities promotes the accumulation of such electrons. Hence it is possible to cool carriers by light through the agency of direct band-to-band transitions. For this purpose it is necessary (when the energy of scattering via interelectron collisions is negligible compared to such scattering of photocarriers by optical phonons) to excite the photoelectrons with a ﬁxed initial energy εi greater than ε0 by utilizing light of such a wavelength that, after the emission of n optical phonons, the photocarriers should have a ﬁnal energy εf < εi . COLD WORKING

COLD CATHODE

Unheated cathode emitting electrons by means of eld emission of electrons. These are e ldemission cathodes, and there are also various types of cathodes emitting nonequilibrium electrons excited by an internal ﬁeld: dispersed metal

Industrial term no longer used much. It means hardening of a metal under the action of cold plastic deformation, but not strain hardening (see also Work hardening). Cold working in optimal mode increases hardness and yield limit, resistance to fatigue deformations, and a decrease of plasticity and

COLLECTIVE EXCITATIONS IN SUPERCONDUCTORS

impact strength. It is used in technology for surface hardening of work pieces with the help of

steel- or cast iron-shot blasting impact treatment, rolling, etc. COLLAPSE OF ELECTRON ORBITS

A sharp decrease of the average radius of an electron orbit in an excited atom occurring for a small change of the nuclear charge (atomic number), Z. The collapse of electron orbits takes place when the screened electrostatic potential −U (r), acting on the electrons and the orbital or “centrifugal” potential 2 l(l + 1)/(2mr 2 ) (where r is the distance from the electron to the nucleus, l is the orbital quantum number, and m is the electronic mass) approximately compensate for each other. Then the effective potential U eff = −U (r) +

2 l(l + 1) 2mr 2

can exhibit two valleys or minima, one near the atom nucleus (at r ≈ a B , where a B is the Bohr radius), and the other at the atom periphery (at r ≈ 10a B ), separated by a positive potential barrier. The deepening of the internal well with increasing Z at a given l results, at a certain critical value of Z = Z c (which depends on l, and also on the electron conﬁguration and on the level), in the redistribution of electric charge density from the outer valley into the inner one, which is interpreted as an electron collapse. This collapse of electron orbits is possible for electrons with l 2. In the isoelectronic sequence of argon-like ions, the collapse of 3d-electrons in the 2p5 3d conﬁguration takes place at Z c = 19, viz., at the transformation from Ar to K+ , while in the isoelectronic sequence of xenon-like atoms the collapse of the 4f -electron in the 3d 9 4f conﬁguration takes place at Z c = 55, i.e. at the transformation from Xe to Cs+ . If the atom or ion is present in a solid then the orbits that did not collapse strongly overlap with neighboring atomic coordination spheres, and the corresponding electrons often become delocalized. Photoabsorption spectra reﬂect the participation of such states, and provide information on the electronic structure of such a solid (see Fine structure of X-ray absorption spectra).

189

COLLECTIVE EXCITATIONS

Motions in a system with a large number of interacting particles associated with the excitation of some collective degrees of freedom, and manifesting themselves in a cooperative dynamics of all the particles (see Phonons). The collective excitations are not necessarily associated with mechanical displacements of the particles: they may be, e.g., electronic excitations in atoms (see Excitons) or excitations of magnetic (spin) degrees of freedom (see Magnons). The collective excitations in condensed media propagate as an ensemble of waves, each of them representing a certain kind of motion characterized by a velocity and an energy. In quantum theory collective excitations are regarded as quasi-particles, their dynamics being described by the corresponding equations of motion. The collective excitations for weak interactions in a system, when the harmonic approximation is valid, obey the superposition principle and play the part of elementary excitations. Introducing the concept of collective excitations facilitates the treatment of a number of physical properties of weakly excited condensed media. Explaining some of these properties requires taking into account the interactions of the collective excitations, which is equivalent to introducing an anharmonicity into their description. In macroscopic systems with a high degree of excitation the collective excitations become transformed, and they can appear as solitary waves (solitons) or shock waves. COLLECTIVE EXCITATIONS IN SUPERCONDUCTORS

Mutually coupled oscillations of the order parameter and of an electric ﬁeld. At a temperature near the critical (transition) temperature, the existence of weakly damped oscillations of this type with an acoustic spectrum is possible. Such oscillations (experimentally discovered by P.L. Carlson and A.M. Goldman in 1975) show up at frequencies which exceed both the reciprocal energy relaxation time, and the reciprocal lag time for the establishment of an equilibrium distribution of quasi-particles over the branches of the energy spectrum. This collective mode represents oscillations of the population differences between the branches of the energy spectrum. Simultaneously, a longitudinal electric ﬁeld appears in the

190

COLLECTIVE VARIABLES METHOD

superconductor, along with currents of normal excitations and of the superconducting condensate directed opposite to one another, so that there is no net current. The phase velocity of such excitations equals: c = [2ΔDχ(2πT τ )]1/2 , where D = v F l/3 is the electron diffusivity (diffusion coefﬁcient), Δ is the energy gap in the superconductor, τ is a characteristic time of scattering from impurities, T is the temperature, χ is the Gorkov function introduced in the theory of superconducting alloys, v F is the Fermi velocity, and l is the electron mean free path. Another type of oscillation existing in superconductors is an oscillation of the order parameter amplitude which has a resonance character (Schmid mode, A. Schmid, 1975). This is associated with the possibility of a virtual decay of Cooper pairs, which requires an energy input of 2Δ. This process involves violation of the energy conservation law and, in accordance with the quantum-mechanical uncertainty principle relating energy and time, must proceed for times of the order of /(2Δ). The amplitude of the order parameter perturbation oscillates with a frequency ω = 2Δ/, and tends toward its steady-state value with a power law dependence on the time. Inelastic scattering mechanisms can bring about an exponential decay of such oscillations. In a hypothetical superconductor treated as a superﬂuid Fermi liquid there are weakly damped oscillations of the phase of the order parameter which have an acoustic spectrum (Anderson– Bogolyubov mode). However, an excitation of the electron density accompanies these oscillations, hence, their frequency is increased up toward the plasma frequency in real superconductors because of Coulomb interactions. COLLECTIVE VARIABLES METHOD

A method of statistical physics that introduces long-range interactions into the thermodynamic and structural properties of multiparticle systems. The description of interacting particles (e.g., atoms, ions or molecules) using collective variables is based on an extended phase space consisting of individual particle coordinates and collective variables associated with the waves of density ﬂuctuations of a certain system parameter (see Fluctuations of atomic positions). Depending on the speciﬁc problem, the latter may be the den-

sity of the number of particles, density of electric charge, spin density, etc. In the simplest case of a single-component system, the collective variables will be deﬁned by means of the Fourier components of the operator of the number density of particles: N 1 exp(ik·r j ), ρ k = √ N j =1

k = 0,

(1)

where r j are the coordinates of the j th particle, and N is their total number. The condition k = 0 √ excludes the constant term ρ k=0 = N δk,0 . The transition to an expanded phase space that includes individual coordinates, {r} = (r 1 , . . . , r N ), and collective variables, {ρk }, is effected via a transfer function which is a product of corresponding δ-functions. Hence, e.g., the system conﬁguration integral can be represented as follows: (2) QN = Q0N (dρ)J (ρ) exp −βθ(ρ) , where Q0N is the conﬁguration integral of the subsystem with short-range interactions, the function 1 (dr) exp −βU0 (ρ) J (ρ) = V N Q0N δ(ρk − ρ k ), (3) × k=0

is the Jacobian of the transition to collective coordinates, the differential factors have the form (dr) =

N j =1

dr j ,

(dρ) =

dρk ,

k=0

where β = 1/(k B T ) is the reciprocal temperature of the system, U0 (r) is the potential energy of the short-range interactions, and the function θ(ρ), given by θ(ρ) =

N N2 ν(k)(ρk ρ−k − 1) + ν(k = 0), V 2V

k=0

(4) is the representation in collective variables of the potential energy of long-range pair inter-particle interactions, ν(k) = dr e−irk Φ(r) is a Fourier component of the long-range potential Φ(r), and V is the system volume.

COLOR CENTERS

A similar transformation to collective variables also can be brought about by means of an integral transform of the Gaussian factor exp[−βθ(ρ)]. The method of collective variables is used to describe the properties of a variety of real systems. Thus, an ion-molecular approach in the theory of electrolytic solutions, based on an equivalent account of the interactions of all the particles in solution, has been developed within the framework of collective variables. This method, supplemented by the density matrix shift transformation, has been successfully employed in the theory of quantum Bose- and Fermi-systems, in particular for constructing a theory of liquid 4 He and describing the electron gas in metals (see Bose–Einstein statistics and Fermi–Dirac statistics). Variables associated with the order parameter of the system have been introduced into the set of collective variables in the theory of secondorder phase transitions, and the explicit form of the transfer Jacobian, J (ρ), is of a non-Gaussian character for three-dimensional systems. In another approach, the collective motions of systems of interacting particles are treated by the canonical transformation method, whereby a transition is made to collective coordinates and momenta that correspond to collective oscillations, or to the elemental excitations associated with them. Since the collective coordinates and momenta are not conventional variables, a transition to them involves additional conditions that conserve the total number of degrees of freedom in the system. COLLISION CASCADE

The avalanche-like process of dislodging (displacement of) atoms (ions) from the sites of a crystal lattice (or of an amorphous solid). The collision cascade arises after energy transfer to the target atom by an external particle as a result of sequential collisions of atoms in the vicinity of the initially displaced one. If the energy of the initially displaced atom is ε, the collision cascade occupies the spatial domain of size l(ε), where l(ε) is the mean free path as a function of its energy. The cascade time is 10−14 –10−13 s; where the cascade over a domain of enhanced concentration of radiative defects arises with its central part enriched with vacancies, and the peripheral one enriched with

191

interstitial atoms. The primary relaxation of a cas-

cade takes ∼10−13 –10−11 s, with some interstitial atoms returning to their initial sites. Then the secondary stage of relaxation occurs, controlled by thermally activated processes (primarily by diffusion). On irradiation with dense beams or with radioactive decay, spatially uniform collision cascades can arise, their only common quantitative characteristic being the cascade function or the radioactive damage function ν(ε). It equals the total number of atoms (ions) displaced from the sites of the solid body lattice by the initial atom with energy ε. Low-energy cascade: ε < εc , where εc is the critical energy, with negligible retardation of the moving atom by electrons below it. All the energy of the atom goes to displace atoms from lattice sites, so that αε (ε < εc ), ν(ε) = εd where εd is the energy for creating a stable vacancy–interstitial atom pair, and α is a factor on the order of unity. As commonly assumed, εd ∼ 25–80 eV, α ∼ 0.4–1. Theoretical values of εc are 0.1 MeV for Fe and 3 MeV for U . For a high-energy cascade: ε > ε c . The retardation of atoms down to energy εc occurs mainly due to electrons of the medium, i.e. without dislodgment of new atoms. Therefore, ν(ε) =

α εc εd

(ε > εc ),

where α is a factor on the order of unity (it can differ somewhat from α). See also Seeger zone. COLLISION IONIZATION See Impact ionization. COLLISION RADIATION See Bremsstrahlung. COLOR CENTERS, F -centers Point defects with optical absorption in the transparent region of a defect-free crystal. Color

centers are related to either impurities (impurity color centers), or intrinsic structural defects in crystals (intrinsic color centers). The main methods to stimulate the formation of color centers are

192

COLORED SYMMETRY

vacancies). Color centers are also found in glasses (see Vitreous state of matter), e.g., a non-bridging oxygen atom in vitreous quartz (band with a maximum at 4.75 eV). The main applications of color centers in practice are lasers, photopigments, dosimetry, and diagnostics of minerals. COLORED SYMMETRY

Color centers.

doping, deviation from stoichiometric composition, and irradiation by ionizing radiation. Electronic transitions that determine the color center absorption are shown schematically in the ﬁgure. Transitions 2 and 3 produce, as a rule, wide absorption bands; transitions 1 give either narrow or broad bands, depending on the magnitude of the electron–phonon interaction. Transitions 4 are observed only under high-power pulse excitation with the aid of time-resolved spectroscopy. Reverse transitions may proceed with photon emission; in this case a color center is simultaneously a luminescent center. Many color centers involve a point defect that has trapped an electron (electron color centers) or a hole (hole color centers). The association of elementary defects (vacancies, interstitial atoms, impurity atoms, or impurity ions) results in the formation of aggregate color centers. An increase in temperature and illumination in the absorption bands of color centers may lead to the release of trapped electrons or holes, i.e. to the destruction (discoloration) of color centers. The most widely studied color centers are in ionic crystals, in particular, in alkali-halide crystals. For example, F -centers (anionic vacancy with a trapped electron, named from the German word “Farbe” for “color”) produce an intense absorption band in the visible region, which corresponds to a transition similar to the 1s–2p transition in a hydrogen atom (F -band), and weaker K-, L-bands refer to transitions to higher F -center excited states. Also H -centers (interstitial atoms of halide X0 ), and Vk -centers (self-localized holes X− 2 ), produce broad bands in the ultraviolet region. In covalent crystals, the absorption of color centers typically occurs as narrow lines, e.g., GR1 and ND1 centers in diamond (neutral and negatively charged

A theory of generalized symmetry of material objects (media and structures), which combines the global symmetry of the system as a whole with the local symmetry of its structural elements. Depending on the method of combination of the groups of global (external) G- and local (internal) P -symmetries, the following colored symmetry groups are distinguished: (1) P -symmetry groups, which are subgroups G(p) ⊆ P × G of the direct products of groups P and G; (2) Q-symmetry groups, which are subgroups G(q) ⊆ P λG of the semidirect products of P and G; (3) Wp -symmetry groups G(Wp ) ⊆ Pwr G = P G × G, which are subgroups of the wreath product (for groups G(Wq ) – of twisted wreath product) of P and G, where P G is the direct product of groups P , taken nG times, n = |G| is the order (or power) of the group G: P G = P g1 × P g2 × · · · × P gn , and the elements gi ∈ G indicate the position of each individual group P in the n-fold direct product. These groups differ in the manner of their effect on a mass point, and in the multiplication law of their elements. In terms of physical interpretation, the lowest groups G(p) and G(q) , isomorphic to the groups G, describe the magnetic exchange symmetry of the structures of magnetically ordered crystals. Groups G(Wp ) and G(Wq ) ↔ G, involving the effect of translation on a mass point (depending on its coordinate), describe the symmetry of real crystals, including quasi-crystals (icosahedral phases), and polysystem molecular crystals with so-called “super-Fedorov” symmetry. COLORED SYMMETRY GROUP

In the general case the subgroups of the direct products (P × G) and the semidirect products (P λG) of groups of external (global) G and internal (local) P symmetries, as well as subgroups of the wreath product Pwr G = P G λG, which operate over subspaces of geometrical coordinates

COMMENSURATE STRUCTURE

193

r ∈ R(3), and of their nongeometrical (“colored”) ◦

counterparts S ∈ S(d). According to the laws of multiplication and to the action of combined elements (p, g) or . . . p(r k ) . . . |g, p ∈ P , p(r k ) ∈ P qk r 1 = P rk ⊂ P r1 × · · · × P rk × · · · = P G of ◦ the material point (S , r), groups of four types are singled out; of global action: ◦ ◦ ◦ P : (p, g) S , r = pS , gr = S , r , (pi , gj )(pk , gl ) = (pi pk , gi gl ) ∈ G(p) ⊂ P × G, ◦ ◦ ◦ Q: (p, g) S , r = pg S , gr = S , r , (pi , gj )(pk , gl ) = pl gj pk gj−1 , gj gl ∈ G(q) ⊂ P λG and of local action – depending on the coordinate ◦

r k = gk r 1 of the point (S , r k ): ◦ ◦ Wp : . . . p(r k ) . . . |g S , r k = p(r k )g S , gr k , . . . pj (r k ) . . . |gj . . . pl (r k ) . . . |gl = . . . pj (r k )pl (r k ) . . . |gl gl , ◦ ◦ Wq : . . . p(r k ) . . . |g S , r k = p(r k )g S , gr k , . . . pj (r k ) . . . |gj . . . pl (r k ) . . . |gl = . . . pj (r k ) gj pl (r k )gj−1 . . . gj gl . The colored symmetry groups are closely connected with the theory of so-called ﬁber SR-spaces (SR ⊂ S(d) × R(3), or SR ⊂ S R (d) × R(3)), and n = (d +3)-dimensional groups, which are their generalized projections onto the threedimensional space. The colored symmetry groups are used to describe magnetically ordered crystals (see Magnetic symmetry group). See also Colored symmetry. COLOR GROUP See Shubnikov groups.

Curves of hardness versus layer depth for different combined heat treatment techniques: nitration or nitrocementation chemical heat treatment (N), and electrocontact (E), induction (I), and laser (L) high-speed hardening.

out, and values of the technological parameters being used. Multiple combined heat treatment techniques allow the variation of properties corresponding to different requirements for surface layers and internal bulk (core) material. Schematic curves of hardness as a function of layer depth are presented in Fig. as an example, where the lower solid curve is a thermo-chemical treatment employing nitration or nitrocementation (N), and the remaining curves represent high-speed hardening via electrocontact (E), induction (I), and laser (L) processes. It is possible to improve hardness and other mechanical properties in near-surface regions, and depending on the methods of heating, at different distances from the surface, taking into account structure and microstructure variations. It is also possible to obtain gradients of particular properties needed for speciﬁc loading conditions. As examples of how metals can undergo combined heat treatments we refer to prior quenching with tempering before thermo-chemical treatment at low temperatures; cementation; nitrocementation with hardening, etc. COMMENSURABLE STRUCTURE See Commensurate structure.

COMBINED HEAT TREATMENT

COMMENSURATE STRUCTURE, commensurable structure

The heat treatment of materials including combinations of heat with chemical and mechanical modes. The choice of combined techniques takes into account the loading conditions, detailed geometry, sequence of operations being carried

A long-period structure, which arises from periodic distortions of an initial lattice due to displacements of atoms from equilibrium positions. The commensurate structure is generally formed during lowering of the temperature at a phase

194

COMPACTION

transition. In a number of cases the system undergoes a sequence of phase transitions to various commensurate states (with sequential variations of the superlattice constant), until reaching the ﬁnal commensurate phase which has a period a that is a multiple of the initial lattice constant a, i.e a = na, where n is an integer (so-called “devil’s staircase”). The transition from the initial structure to a commensurate one proceeds in certain materials through an intermediate temperature incommensurate structure, with a superstructure constant incommensurate with the lattice constant of the initial phase (see incommensurate–commensurate phase transition). The commensurate structure may be represented as modulated by shear waves, e.g., charge density waves (spin density waves), in one, two or three directions; with the modulation period determining the displacements of atoms from their initial equilibrium positions. The periodicity of the new structure is fully commensurate with that of the initial structure: Q = nq, where Q and q are wave vectors of the commensurate and the original structures, respectively, and n is an integer. The translational symmetry is not violated in the generation of the commensurate structure. The commensurate structure can be detected by diffraction methods, e.g., through an electron diffraction observation of extra reﬂections corresponding to basic structure reﬂections for multiple distances, and by changes of other physical characteristics: electrical resistance, magnetic susceptibility, Young’s modulus, etc. The commensurate structure occurs in dichalcogenides of transition elements MX2 (M = Ta, Nb; X = Se, Te, S), in crystals of the A15 and cubic Cu2 Mg types, in the premartensitic region of temperatures in a number of compounds based on equiatomic TiNi, in Cr, etc. COMPACTION

See Pressing. COMPENSATION

See Conductivity self-compensation, Ionic conductivity compensation, Magnetic compensation.

COMPENSATION RULE, Meyer–Neldel rule (W. Meyer, H. Neldel) A relationship between the activation energy

E and the preexponential factor σ0 in the temperature dependence of the electrical conductivity σ of semiconductor:

E . (1) σ (T ) = σ0 exp − 2kB T The analysis of many experimental data obtained for semiconductors possessing current carriers with small mobilities has shown that lg σ0 = α E + β.

(2)

Here α and β are parameters characteristic of the material. Eq. (2) represents the compensation rule which has been widely investigated for polymeric semiconductors. This is explained with the help of the charge transport tunnel model (see Tunnel effect). COMPLEX ELASTIC MODULI Tensor factors in Hooke’s law written for harmonically time-varying stresses and strains in disω = sipative media (see Dissipative structures): σik ω , where σ ω and ε ω are Fourier comciklm (ω)εlm ponents of stresses and strains, respectively. The imaginary part of the complex elastic modulus, called the loss modulus, is responsible for the damping of elastic waves in a medium.

COMPLEXY

A thermodynamic equilibrium defect in a solid solution consisting of an impurity atom complex located at a group of lattice sites whose number differs from the number of complexy atoms. The concept of complexy was introduced by M.A. Krivoglaz (1970). It can be energetically advantageous to form a complexy from atoms with strongly differentiated atomic radii if this results in a partial removal of stresses and a decrease of the overall elastic energy. A complexy is less advantageous from the entropy standpoint than isolated impurity atoms, and the complexy concentration in a solid solution decreases with temperature in contrast to the behaviour of point defects. Complexy formation radically affects the temperature and concentration dependences of crystal lattice

COMPTON EFFECT

constants, diffusion coef cients, solubility of impurity atoms, diffuse scattering of X-rays, and other solution characteristics. A noticeable change in lattice parameters should be observed in alloys containing complexies, and these parameters are detected by dilatometric analysis and X-ray diffraction techniques. Complexies have been detected experimentally in a lead–gold alloy. COMPOSITE MATERIALS (fr. Lat. compositio, combination)

Materials consisting of two or more components with a distinct boundary between them, and possessing properties not found in the individual components taken separately. Anisotropic and isotropic (quasi-isotropic) composite materials are distinguished. Among the ﬁrst are reinforced composite materials including matrix and reinforcing components in the forms of ﬁbrils, wires, threadlike crystals, strips, and grids oriented in it in a predeﬁned fashion. There are metallic, polymeric and ceramic composite examples differentiated by the matrix type. Among the second are precipitationhardened materials, pseudoalloys, and randomly reinforced composites. The dispersion-hardened varieties have a matrix structure consisting of a basic material with ﬁne dispersed hardening inclusions; the pseudo-alloys can have the structure of interpenetrating skeletons, a statistical powder mixture, or a matrix structure depending on its composition and formation process; randomly reinforced materials have a matrix structure with no preferred orientation direction of ﬁbrils or inclusions. Reinforcing ﬁbrils and inclusions endow composite materials with strength, hardness, and the matrix with bonds between components, load transmission on ﬁbrils, and corrosion resistance. Properties of composite materials depend signiﬁcantly on phase boundary strength, hardening components, their size and quantity. One of the main requirements imposed on composite materials used for construction is the lack of signiﬁcant diffusion (see Diffusion) and chemical interactions of the components during the preparation and high-temperature use. By varying the structure and composition it is possible to modify the strength characteristics over a wide range, fracture toughness, electrical conductivity, thermal expansion factor, and other properties.

195

COMPOSITE MATERIALS, STRENGTH See Strength of composite materials. COMPRESSIBILITY, volume compressibility factor

Relative variation of the volume of a body under the effect of total pressure. One can distinguish the isothermal volume compressibility, κT = −(∂v/∂p)T /v = −((∂ ln(∂Φ/∂p)T )/∂p)T (Φ is thermodynamic potential) and the adiabatic volume compressibility, κS = −(∂v/∂p)S /v = −(∂v/∂p)T /v − T vα 2 /cp (where cp is the speci c heat of the body under constant pressure, α is the volume coefﬁcient of thermal expansion). The isothermal compressibility exceeds the adiabatic one for the majority of solids by not more than several percent. The compressibility has the units m2 /N = 1/Pa (typical value is ∼1/GPa). COMPRESSIBILITY MODULUS The same as Bulk modulus. COMPRESSION, UNIFORM See Uniform compression. COMPTON EFFECT (A. Compton, 1922) The scattering of an X-ray or gamma quantum off a free (or weakly bound) electron to which the photon transfers a part of its energy

and momentum. The change of the photon wavelength λ at scattering is determined by the energy and momentum conservation law and is equal to

λ = λ − λ0 (1 − cos θ), where λ is the wavelength of the scattered photon, λ0 = h/(mc) is the Compton wavelength equal to 2.426·10−12 m, θ is the angle between the directions of motion of the incident and scattered photons. The scattering intensity evaluated by quantum theory provides the angular distribution of scattered photons (mainly forward scattering) and the scattering cross-section σ which depends on the photon energy ε, with σ (ε) decreasing with ε. In the limit ε → 0 we have σ → σT = 8πr02 /3 (r0 is classical electron radius, r0 = 2.8·10−15 m). The Thomson’s scattering cross-section σT was derived by J. Thomson in the classical theory of electromagnetic wave scattering. The Compton effect can occur for scattering off other charged particles as well, but the effect is seen only for high-energy

196

COMPUTATIONAL MICROTOMOGRAPHY

photons scattering off particles with large masses. If the electron involved in the Compton scattering has a high velocity then an increase in photon energy is possible at scattering (inverse Compton effect). The Compton effect gives a strong contribution to the generation of fast electrons in gamma ray irradiated solids, and these generated electrons create radiation defects through impacts with target atoms. COMPUTATIONAL MICROTOMOGRAPHY

A method of scanning an object with a probe of penetrating radiation and, with the aid of a computer, subsequently reconstructing an image which contains details of the internal microstructure of the object in a series of thin layer cross-sections. Ordinary transmission images, being two-dimensional shadow projections of the actual three-dimensional object, do not give signiﬁcant information about its internal structure, because they display information averaged according to the thickness. In contrast to this the digitized images called tomograms (see Tomography) provide considerably sharper differentiation of areas with differing absorption coef cients, and better separation of the images of overlaying structures. To apply computational microtomography the object is transilluminated with a narrow beam of the penetrating radiation (e.g., X-rays, electrons, ultrasound, or IR) and the radiation that passes through it is recorded by corresponding detectors. By sequentially scanning the beam and/or turning the sample, a set of projection data necessary for reconstructing the tomogram is obtained. The result is a sequence of two-dimensional halftone cross-section images, and the data from these cross-sections can be used to reconstruct a threedimensional image which reﬂects the true microstructure of the object. Microtomography has been successfully used in transmission electron microscopy for the investigation of molecules, bacteriophages and membranes (with spacial resolutions of angstroms), in scanning electron microscopy, and in optical and X-ray microscopy for investigating the properties and structure of solids with dimensions of about 1 mm and resolutions of micrometers. The technique is also used in the non-destructive defectoscopy of components of solid-state quantum

electronics, providing visualization and identiﬁcation of the subsurface micro-structure and defects. See also Tomography of micro e lds. COMPUTER ALGEBRA

A process in applied mathematics and computer engineering, that uses computers for the automation of symbolic derivations. Computer algebra is designed for the execution of cumbersome (routine) analytic manipulations that cannot be readily carried out manually: multiplication (division) of polynomials, cancellation of similar terms, formation of an arbitrary algebraic expression with respect to a dependent variable, substitution of variables, integration, differentiation, etc. This approach can facilitate and improve the accuracy of subsequent numerical calculations, provide analytical relationships between various parameters, and overcome difﬁculties involved in the subtraction of nearly equal large magnitude numbers. COMPUTERS in solid state physics

Various methods for applying computers to solve problems in the ﬁeld of solid state physics. In experimental solid state physics a computer performs the following three functions: control of apparatus (e.g., the control of devices designed for molecular beam epitaxy when synthesizing superlattices); data analysis (such as deciphering various spectra); planning experiments. In an optimal situation, all these functions are coordinated, so that the computer performs quite a complicated range of research tasks. In analytical solid state physics most of the important applied problems, as well as an ever-growing share of the fundamental problems, are solved using computers. Two approaches are dominant in this ﬁeld: the numerical solution of equations, and the direct modeling of observed solid state phenomena with the help of computers (see also Computer simulation). The ﬁrst approach of solving systems of equations is not speciﬁc for solid state physics, and its efﬁciency is determined, to a great extent, by the capabilities of the computer. For single-processor computers the absolute or theoretical limit of their productivity is about 109 operations/s, but in practice the limit is lower by one or two orders of magnitude. For a relatively simple problem, such as a

COMPUTER SIMULATION

study of the initial stages of monocrystal growth from an atomic beam at a perfect monocrystal face, it is necessary to analyze a Markovian chain consisting of hundreds or (at low saturation in the vicinity of the critical point) a few thousand nonlinear differential equations. The determination of the distribution function of the atomic groupings for any given set of initial conditions requires the performance of about 108 operations/s. For a reasonably complete analysis involving the entire range of available growth conditions one needs to perform 1010 or more operations/s. The problem becomes too difﬁcult for multicomponent crystals, and indeed insoluble for single-processor computers when the ﬁnal growth stages are included in the calculation. Multiprocessor computers are also inefﬁcient in the framework of the ﬁrst approach, because extensive parallelism of the data processing is hardly achievable. In contrast, the second approach of modeling observed phenomena is quite compatible with the architecture of multiprocessor computers. The real space of the crystal can be divided into a network of conventional cells (hence the term network models) and a step-by-step analysis of changes in the states of cells and their interactions can be carried out. In the extreme case, a cell is represented by an individual atom (e.g., Ising model). The organization of this modeling system can be either linear, two-dimensional, or threedimensional. A conformity between the computational process and the processes occurring in solids is provided by means of both the programs and the apparatus. The former are universal (because the program approach allows one to model any physical process using any computer) but they do increase the duration of each step of the modeling. The latter (i.e. the apparatus part) speciﬁes the computer for each individual problem, and provides for its rapid solution. In the extreme case, the relations between the processors of the modeling system are isomorphous to the relations in the modeled solid; and the productivity increases as the number of processors increases. There exist modeling systems (so-called distributed matrix processors, “hypercube”) consisting of 105 (in order of magnitude) processors. Theoretically it is possible to produce such systems containing up to 1012 modeling processor units with a clock period

197

to 10−9 s, which permit the solution of a large part of the problems of solid state physics in real time. Further progress depends, in principle, on creating new solid and molecular modeling systems that implement the probability functions at the quantum level. In terms of the complexity of the modeling, the problems of solid state physics could be classiﬁed as follows: (i) crystallization and recrystallization in the absence of continuous defects; (ii) the same processes with the participation of dislocations and other continuous imperfect defects; (iii) electronic, thermal, and diffusion (see Diffusion) processes with changes in the location of internal boundaries (e.g., semiconductor junctions); (iv) non-structural phase transitions; (v) ﬁrstorder structural phase transitions with alteration of the lattice symmetry; (vi) second-order structural phase transitions; (vii) modeling processes on a “rigid” lattice with a quantum-mechanics analysis of elementary events; (viii) subsequent quantummechanical analysis of processes in solids with changes of lattice symmetry. At present, models of the former four types are really quite welldeveloped, and the efﬁcacy of the latter four types depends on future progress. COMPUTER SIMULATION, computer modeling

Investigation of structures and phenomena by their information simulation on computers. Direct simulation is achieved by an organization of elements of the computer and the topology of communications between them such that the properties of data-regulated processes are similar to the corresponding characteristics of the object. In this case, the maximum performance of the simulation process is achieved, but each structure and each type of phenomena need a special machine (or its complicated adjustment). Alternatively simulation is carried out by numerical treatment of mathematical equations describing the object at various boundary and initial conditions. The similarity to the object is achieved only by means of software. The hardware of simulation is universal but its efﬁciency (even at the maximum speed of the elements) is rather limited. Historically, the ﬁrst simulation was performed by analog machines for physical processes formally described by the same equations as the phenomena under

198

CONCENTRATION

study. Now there are analog machines based on various physical phenomena (transients in electric circuits, optical and acoustic waves, processes in solids and on their surface, etc.). They allow one to carry out a parallel multichannel simulation in the real-time mode of a physical process achieving an effective capacity up to and even more than 1010 –1011 operations per second. The physical structure and manufacturing techniques of such devices are relatively simple, and the energy consumption is minimal. However, besides the specialization, their shortcoming is low accuracy of calculations and instability of the simulation process. Computer simulation by numerical solution of the equations describing a physical object possesses quite opposite features. There are two approaches to computer simulation combining the advantages of digital and analog principles. The ﬁrst is based on multiprocessor computers (see Computers in solid state physics). In this case, a similarity is reached between the organization of ﬂows of the internal information exchange in a computer and mass–energy ﬂows in a modeled system. The performance of computer simulation increases by several orders; under optimal conditions, proportional to the number of processors in the system. Another approach is based on joining digital and analog processors in one device (so-called hybrid devices) in which, at each stage of simulation, the optimal distribution of data ﬂuxes between digital and analog subsystems is realized. The analog subsystem provides the maximum speed of analysis of special problems arising during simulation, and the digital one provides stability and universality of simulation, and the accuracy of the calculated data. Both approaches (digital multiprocessing and digital–analog hybrid) are based on the development of microelectronics and an increased integration of computer elements. In prospect, supermultiprocessor (up to 109 –1011 modeling cells) hybrid devices will unite the advantages of all the above-mentioned approaches to computer simulation. CONCENTRATION

The relative content of a component in a system (solution, mixture, melt). There are many different ways of expressing this: mass, moles, volume fraction, relation of individual mass or individual moles to the total. These concentrations

can be expressed as fractions, as mass or volume percentages (%), or for high dilutions as, e.g., parts per million (ppm) or parts per billion (ppb). Other ways for expressing the amount of a component and the amount of a total system are: mass concentration – the relation of the component mass to the system volume (kg/m3 , more often g/l); molar concentration (molarity) – the relation of the component quantity in moles to the system volume (mol/m3 , more often mol/l); molal concentration (molality) which is the relation of the component quantity in moles to the solvent mass (mol/kg); normal concentration (normality, n) – the number of gram-equivalents of the substance in one liter of solution; titer – the number grams of the component dissolved in 1 ml of the solution. The last two quantities are common in analytical chemistry. Furthermore, in the literature concentration is sometimes expressed as mass of the component being dissolved in 100 g of solvent, or as number of moles of the component in 1000 moles of solvent. The SI system recommends using only mass and molar concentrations. CONCENTRATION-DEPENDENT PHASE TRANSITION A phase transition characterized by the spon-

taneous onset of long-range order at T = 0 (see Long-range and short-range order) at a change in concentration of the repetative units forming

the crystal. Depending on the physical nature of the associated order parameter that arises, such a phase transition can be ferromagnetic, ferroelectric, structural, etc. Let us consider for deﬁniteness the ferromagnetic concentration-dependent phase transition in a system in which magnetic atoms replace nonmagnetic ones in a random fashion. Because the exchange interaction rapidly decreases with distance it is possible to consider as a ﬁrst approximation that only nearest neighbor magnetic atoms are interacting. At absolute zero temperature all magnetic moments coupled by exchange are oriented parallel. If the concentration x of magnetic atoms is small they form clusters isolated from each other with dimensions which do not vary with an increase of the crystal volume (ﬁnite clusters). The average magnetic moment of the whole crystal is equal to zero in this case since various clusters have oppositely directed

CONDENSED MATTER INTERFACE

199

cooling or compression. Condensation is a r storder phase transition. Vapor condensation is only

The dependence of the probability P (x) for the formation of an inﬁnite cluster on the concentration of magnetic atoms x for a simple cubic lattice.

moments. With an increase in x the characteristic size of terminal clusters increases, and at a certain critical concentration xC a cluster forms whose number of particles is proportional to the system volume, the so-called inﬁnite cluster. The magnetic moment of a crystal M(x) for x > xc differs from zero, being equal to M(x) = M(1)P (x), where M(1) is the magnetic moment of the ordered crystal, and P (x) is the probability of the formation of an inﬁnite cluster (one occupation per lattice site). Thus, at x = xc and T = 0 a phase transition from the paramagnetic state to the ferromagnetic state takes place, an effect closely related to percolation (see Percolation theory). Examples of these phase transitions in materials with interacting nearest neighbors are: semimagnetic semiconductors Cd1−x Mnx Te, Cd1−x Mnx Se, insulators SnTex Se1−x , etc. The theoretical dependence of P (x) on the concentration x of magnetic ions for a simple cubic lattice (xc = 0.31) is given in the ﬁgure. At a ﬁnite temperature T the phase transition persists, and its transition temperature Tc (x) approximately satisﬁes the condition Tc (x) = P (x)Tc (1), where Tc (1) is the temperature of the usual phase transition in an ordered crystal.

possible at subcritical conditions. Condensation to the liquid phase occurs if the temperature and pressure are above their triple point values, and it occurs directly into the solid phase if they are lower than the triple point values. The quantity of heat released at condensation is the same as that which was supplied at evaporation or sublimation, processes which are the inverse of condensation. At constant temperature condensation occurs until a vapor–condensed phase equilibrium is established which is described by the Clausius– Clapeyron equation. If the saturated vapor is a mixture of gases then this equation holds for each individual component. For the determination of condensed phases that are in equilibrium with a vapor of complex composition it is possible to make use of the complete phase diagrams. During condensation metastable phases are often formed in which the system can persist for a long time before reverting back to a more stable (at the given conditions) state (steel hardening, amorphous metal formation on cooling). Condensation throughout a volume containing vapor and on a surface are distinguished. During condensation on a cooled surface the velocity of condensing molecules has an important signiﬁcance which depends on several things: the difference between the vapor and the surface temperatures, heat exchange processes, condensation surface (solid or liquid, both continuous and dispersed), the presence of noncondensible gases, etc. The mere presence of a supersaturated vapor is not sufﬁcient for inducing condensation within the vapor volume in the absence of condensed phase particles; it is necessary to have condensation centers available (impurity particles, ions). The formation of an equilibrium nucleus of a new (condensed) phase can be unstable, and is describable by the Kelvin equation. The condensation of a vapor into a crystalline phase occurs during crystallization, epitaxy, or physical and chemical precipitation from the vapor phase. CONDENSED MATTER INTERFACE

CONDENSATION

A transition of a material from the gaseous state to a condensed (liquid or solid) one due to

A layer which separates two materials of different chemical composition that are in contact. One can distinguish geometrical and physical con-

200

CONDENSED STATE OF MATTER

densed matter interfaces. The concept of a geometrical interface is used in describing the physical properties of two bodies in contact when the layer thickness is very small compared to the bulk dimensions of these bodies so it has a negligible inﬂuence on the bulk properties. A physical condensed matter interface is a transition layer of ﬁnite thickness between bulk materials whose chemical composition differs from the chemical composition of the media in contact, and hence it can inﬂuence their properties. One can distinguish sharp and smooth interfaces. A transition layer between contacting media with a thickness the order of magnitude of an interatomic distance is called sharp, and it can be obtained by the molecular epitaxy method. A transition layer much thicker than the atomic scale is called smooth. CONDENSED STATE OF MATTER

Solid and liquid states of matter. The condensed state is characterized by high matter density in comparison with a gas, and by a rather low speed of motion of its component atoms. The regular arrangement of atoms or molecules on a three-dimensional lattice with long-range order (see Long-range and short-range order) determines the crystal structure that corresponds to an equilibrium state. There is only short-range ordering in the arrangement of atoms in a liquid. The structure of amorphous solid bodies is equivalent to that of a liquid; and from the thermodynamic point of view the amorphous state represents a supercooled liquid with a very long relaxation time for transition to the equilibrium crystal state. Macroscopic liquids and amorphous materials are isotropic. Materials intermediate between crystal and amorphous solids are polymers, liquid crystals, quasi-crystals, and the gaseous crystalline state. Polymers consist of periodic linear chains at sites where particular atom groupings are allocated. The chain molecules can be bound together in different ways. The parallel arrangement of polymeric chains deﬁnes the polymer anisotropy (see Anisotropic medium). The properties of liquid crystals are determined by the ordered orientational arrangement of their molecules which are often elongated or disk like in shape, and this results in the anisotropy of liquid crystals. There is only short-range order in the spatial arrangement of the molecule centers.

CONDENSON (fr. Lat. condensatio , densi cation, thickening)

A self-localized state of an electron in an elastically deformed medium, or a hypothetical quasiparticle in a covalent crystal in which all atomic bonds are covalent. An electron induces dipoles in neutral surrounding atoms of a medium, and then by its electric ﬁeld attracts them. As a result of small atom displacements, an increased density region is formed which represents a potential well for the electron (see Electrostriction) where it is localized. A macroscopic consideration of a condenson which takes into account a strain potential shows that if self-localized condenson states are at all possible in homopolar crystals, they will have a small radius. A macroscopic condenson can be realized in three-dimensional homopolar crystals with a “loose” crystal lattice due to weak medium anharmonicities. In onedimensional crystals a condenson can also exist in an harmonic elastic medium. A similar situation is realized, in particular, with the application of a quantizing magnetic eld to a crystal. In crystals with negative electron af nity energy (He, Ne) a reciprocal type of electron self-localization is possible with the formation of a lattice disperse region or even the appearance of a small cavity inside which the electron cloud (|Ψ |2 ) is mainly localized. CONDON APPROXIMATION See Franck–Condon principle. CONDUCTANCE, ELECTRICAL See Electrical conductance. CONDUCTANCE, HIGH-FREQUENCY See High-frequency conductance. CONDUCTION BAND An energy band of a crystal comprising elec-

tronic states with energies higher than those of ﬁlled valence bands. Weak external effects on the conduction electrons can cause a change in their average linear momentum, i.e. induce the appearance of current. To create current carriers in the conduction band of intrinsic semiconductors and insulators it is necessary to overcome an energy barrier, with

CONDUCTIVITY SELF-COMPENSATION

a minimum value called the fundamental gap (see Semiconductors). The gap ranges from about 0.1 to several electronvolts in semiconductors, and can reach about 10 eV in insulators. Typical physical mechanisms of current carrier generation are optical and thermal excitation in semiconductors, and ion collisions as well as electrical breakdown in insulators. The parameters that describe the conduction band are the same as those for the valence band: width, effective mass, presence of Van Hove singularities and their symmetry, and spin–orbital splitting (see Spin–orbit interaction). Methods for studying the conduction band include light absorption, cyclotron resonance, photoeffect, Hall effect (see Galvanomagnetic effects), etc. CONDUCTION ELECTRONS Elementary excitations (quasi-particles) of the electron Fermi liquid of metals which carry electric

charge in transport. Every quasi-particle has the same charge and spin as a free electron (exceptions are double charges (2e) in superconductors, and fractional charges in the quantum Hall effect). In the absence of external ﬁelds, the conduction electrons are characterized by the quasi-momentum p and the energy band number s. Their energy εs (p) is periodic (dispersion law) in respect to p with a period 2πb where b is a reciprocal lattice vector. A deviation of εs (p) from the quadratic isotropic dispersion law of free electrons serves as a source of numerous diverse effects which are particularly pronounced in strong magnetic ﬁelds. At a temperature T much less than the Fermi temperature T F = εF /k B (here εF is the Fermi energy, and for a typical metal, T F ∼ 105 K), the conduction electrons form a weakly-nonideal gas. A speciﬁc contribution of the electron–electron interaction to the inverse lifetime of the conduction electrons with ξ ≡| εs (p) − εF | εF is of the order of ν = (εF /)(ξ/ε F )2 . At ξ → 0, the ratio ν(ξ )/ξ → 0 which means that conduction electrons at low levels of excitation ξ εF behave as long-lived quasi-particles. This is the basis for the Landau theory of Fermi liquid describing the electronic properties of normal metals. CONDUCTIVE CHANNEL, SURFACE See Surface conductive channel.

201

CONDUCTIVITY See Electrical conductivity, Effective electrical conductivity, Electronic conductivity. Fröhlich conductivity, Hopping conductivity, Intrinsic conductivity, Ionic conductivity, Surface electrical conductivity. CONDUCTIVITY SELF-COMPENSATION A process of electrical conductivity compensation in doped semiconductors when additional

compensating defects are formed as a result of introducing free current carriers (conduction electrons, holes) into the semiconductor. The formation of the inherent compensating defect during the self-compensation may be stimulated by the introduction of impurity donor or acceptor atoms, as well as by injection of carriers through the contact or by their formation under the effect of light on an intrinsic semiconductor. Self-compensation of conductivity is effective in the case when some of the inherent defect types in semiconductors have sufﬁciently deep acceptor levels (for n-type semiconductors) or analogous donor levels (for p-type semiconductors) that the energy outlay W for thermal formation of the defects of the given type is almost completely compensated by the energy gain E in the trapping of a free carrier to the level of the forming defect. As the defect formation leads to the growth of crystal entropy S, at a sufﬁciently high temperature T and small energy difference (W − E) the minimum free energy of the crystal F = E − T S (E is the Helmholtz energy of the system) may be attained at defect concentrations ND comparable to the concentration of the carriers being introduced. Here, in the state of thermodynamic equilibrium, the actual concentration of current carriers may be signiﬁcantly lower than the concentration of impurities of donor and acceptor types with shallow levels (low ionization energies). It is not possible to obtain high conductivity over the entire series of semiconductor materials (e.g., n-Cu2 O, p-CdS, alkali-halide crystals, etc.). The kinetics of selfcompensation of conductivity is determined by the probability of the elementary act of defect formation, stimulated by the trapping of the charge carrier at a deep level during the course of defect generation. If conductivity self-compensation occurs under conditions involving the exchange of atoms between the crystal and its environment

202

CONDUCTIVITY, THERMAL

(high temperatures, pressures), then vacancies or impurity interstitial atoms may be the compensating defects. CONDUCTIVITY, THERMAL See Thermal conductivity and Thermal conductivity coef cie nt. CONDUCTIVITY, THERMALLY STIMULATED See Thermally stimulated conductivity. CONDUCTORS, electrical conductors

Materials with low speciﬁc electrical resistance (resistivity, usually below 10−6 ·m). Conductors include, for example, metals, metal alloys, semimetals (including graphite). The current carriers (charge carriers) in solid conductors are ordinarily conduction electrons. Typical for a conductor in its normal (not superconducting) state is the linear dependence of the current density on the strength of the applied electric ﬁeld (Ohm’s law). Identifying conductors as a separate class of materials can be somewhat subjective since conductivity depends on many factors, including temperature. For example, many (poor) conductors transform to a superconducting state at extremely low temperatures. CONFIGURATION INTERACTION

Interaction of multiparticle states (conﬁgurations) described by wave functions constructed

from single-particle states (see Slater determinant). The matrix elements of this interaction operator were found by J.C. Slater (1929) for orthogonal, and by P.O. Löwdin (1955) for nonorthogonal single-electron functions. The conﬁguration interaction decreases the total energy of a fermion system by the so-called correlation energy. It is necessary to take the conﬁguration interaction into account for systems with uncompensated electronic spin (atoms, ions, radicals, impurities with partially ﬁlled d- and f -shells in crystals, etc.), that is systems with unﬁlled shells. From considering a set of multiparticle conﬁgurations as the basis for solving the multielectronic Schrödinger equation, and utilizing its linearity, one arrives at the method of second quantization which is a more convenient one for treating a large number of particles. Applying the conﬁguration interaction in solids results in the narrowing of the electronic bands obtained from solutions of the Hartree– Fock equations (see Hartree–Fock method). CONFOCAL DOMAIN, focal conic domain A domain defect in a structural liquid crystal (smectic liquid crystals A, C, cholesteric liquid crystals) which has the form of a cone of rev-

olution. Because of the different orientations of molecules on the liquid crystal boundary the layers inside the confocal domain are curved with their shapes determined by the condition of maintaining an invariable width of each layer. The layers with Dupin cyclides fulﬁll this condition, as shown in Figs. 1 and 2. This results in the appearance in

Fig. 1. Conﬁguration of smectic layers in a confocal domain of a general form (left) and of a toroidal form (right).

CONFORMATIONS

203

tial spaces free of confocal domains are ﬁlled with layers of a ﬂat or spherical shape. The only discontinuities in the layer wrapping for this ﬁlling are confocal pairs. Confocal domain formation plays an important role in phase transitions and relaxation of mechanical stresses. Polarizing microscopic analysis of confocal domain structure in smectic textures has formed the basis for clarifying the onedimensional stratiﬁed structure of these media. CONFORMATIONS (fr. Lat. conformatio, shape, arrangement)

Fig. 2. Micrograph of an isolated domain in a type A smectic liquid crystal.

the confocal domain of a pair of defect lines on which the layer wrapping undergoes a discontinuity. More often one observes a confocal domain with a pair of confocal ellipses and hyperbolae situated in mutually perpendicular planes. The ellipse is located on the perimeter of the confocal domain base, and the hyperbola passes through the confocal domain vertex. In a domain with a torus conﬁguration of layers the ellipse degenerates into a circumference and the hyperbola into a line. Confocal domains with defects of a parabolic type are known as well. The confocal domain is the main element for extensively ﬁlling the layers in a liquid crystal; in particular they form confocal textures which are most commonly observed in smectics and cholesterics. At the ﬁlling, a system of adjacent confocal domains in contact with each other and of sequentially decreasing sizes is formed; the smaller domains being inserted into the gaps between the larger ones. The minimal confocal domain size is determined by the conditions of molecular orientation near the liquid crystal surface (see Boundary effects in liquid crystals). Intersti-

Different spatial conﬁgurations of a polyatomic molecule which can transform between each other without breaking valence bonds, by executing rotational displacements around single bonds, or by changing bond angles. For example, the ethane molecule C2 H6 which has a C3 symmetry axis joining the carbon atoms, changes its energy by twisting one CH3 group relative to the other in an approximately sinusoidal manner with energy maxima corresponding to D3h point group symmetry when the C–H bonds of the two CH3 groups are aligned, and energy minima corresponding to D3d symmetry when they are staggered. An example of conformations involving crystals is twinning of crystals in calcite CaCO3 wherein it is the possible to transform the unit cell from the form of a skewed prism into a direct prism, and then into a plane-reﬂected one, via a shear strain. The conformation concept is used also in a quasi-molecular deﬁnition of impurity-defect complexes and clusters, which are models of localized regions of a solid. Conformation analysis has been widely applied to cluster models for the determination of macrostructures of random semiconductor (see Disordered solids) surfaces and boundary layers. The local minima on a molecular potential energy surface correspond to stable conformations. The transition between local minima is carried out along a curve designated by K. Fukui (1970) as the path of minimum energy. Regions of multidimensional potential energy surfaces, so-called conformation maps, are useful in practice. In conformation analysis the conformer concept is introduced. It represents a set of conformations which form in the space of independent geometrical variables a continuous region including coordinates of the minimum adiabatic potential, with the region

204

CONICAL REFRACTION OF ACOUSTIC WAVES

under consideration laying below the lowest adjacent ﬁrst-order saddle point. CONICAL REFRACTION OF ACOUSTIC WAVES A special type of acoustic wave refraction on a ﬂat crystal face oriented normally to an acoustic

axis, i.e. in a direction along which a great number of quasi-transverse waves with identical velocity can propagate. An exception is the acoustic axis being coincident with a 4th or 6th order symmetry axis. Conical refraction was observed for the ﬁrst time during the propagation of acoustic waves in nickel crystals (J. de Klerk, M.J.P. Musgrave, 1955) and in dihydroammonium phosphate crystals (K.S. Aleksandrov et al., 1963). Interior and exterior conical refraction are distinguished. For the interior conical refraction the whole cone of acoustic beams corresponds to one wave normal, while for the external conical refraction the whole cone of wave normals corresponds to one beam direction. The angular opening is determined by the crystal elastic moduli and can reach tens of degrees as distinct from conical refraction of light waves. For example, it is 61◦ 30 for a calcite crystal. The special case of conical refraction in the direction of an acoustic axis located in the plane of elastic symmetry of a hexagonal crystal, when the refracted beams are distributed in a fan with a ﬂat section, was predicted by A.G. Khatkevich (1962). Under the conditions of conical refraction several effects have been observed: the reﬂection of a linearly polarized acoustic wave from a free crystal face parallel to the wave vector of an incident wave accompanied by a 90◦ rotation of its polarization plane, acoustic wave refraction on the internal surface of a twinned crystal (see Twinning of crystals), in quartz, and in a number of other ways. At ultrahigh frequencies the observation of conical refraction is complicated by acoustical activity phenomena (see Rotation of acoustic wave polarization plane). CONICAL REFRACTION OF LIGHT WAVES A special type refraction of light in optically biaxial crystals observed during propagation in the direction of any binormal optical axis (see Crystal optics). In conical refraction the thin polarized

light beam which is incident on a face of the planeparallel lamina makes up the beam in the form of

a full cone whose vertex is located at the point of the beam incidence on the face. Thus linearly polarized waves with continuously varying (in the range of 180◦ ) polarization azimuth propagate in directions of cone generators. Conical refraction was predicted by W. Hamilton (1832) and observed by H. Lloyd (1833). Internal and external conical refraction can be distinguished. Internal conical refraction occurs in light beam transmission in the binormal direction, in this case the vertex is located on the forward lamina face; on emerging from the lamina the beam makes up a hollow cylinder. External conical refraction occurs for light transmission in the biradial direction, in this case the cone vertex is located on the output lamina face. If the light beam direction does not coincide with the optical axis direction then ordinary birefringence occurs. CONOSCOPY (fr. Gr. κωνoς , a cone, and σ κoπεω, am looking, am observing)

A method of investigating optical properties of oriented anisotropic media (birefringent crystals) with the help of interference ﬁgures (so-called conoscopy ﬁgures) observed in convergent polarized light beams. In conoscopy polarized microscopes, conoscopes, and gas lasers with polarized devices are used. A conoscopy ﬁgure is obtained for light beams convergent on a birefringent crystal (uniaxial crystal or biaxial crystal) using a crossed polarizer and analyzer. The type of the ﬁgure depends on the number of optical axes of a crystal, the angles between them, the presence or absence of optical activity (see Rotation of light polarization plane), crystal lamina orientation or their combination,

Conoscopy ﬁgures obtained with light beams converging on a single crystal with crossed polarizer and analyzer: (a) for linearly polarized light, and (b) for circularly polarized light.

CONSERVATION LAWS

and polarization of light. For linearly polarized light, conoscopy ﬁgures consist of isochromates and isogyres as shown in Fig. (a). The isochromates form a family of concentric interference rings or bands, each of which corresponds to a particlar phase difference of the interfering waves; in white light the bands have a rainbow coloring. The isogyres are mutually perpendicular brushlike dark bands corresponding to directions of light transmission through the crystal in which the linear polarization is not affected. With circularly polarized light the isogyres are absent, as shown in Fig. (b). CONSERVATION LAWS of quasiparticles

Regularities whereby the values of some physical parameters of materials do not change in time. Most conservation laws existing in physics (energy, momentum, angular momentum, etc.) are applicable to solid state physics, provided the necessary conditions hold. The states of elementary excitations (quasiparticles) in crystals are characterized by a vector, similar to the linear momentum, the quasimomentum k. It is deﬁned to within an arbitrary vector of the reciprocal lattice (k and k describe physically equivalent states, if k − k = 2πb, where b is a vector of the reciprocal lattice). In the interaction of elementary excitations (the collision of quasi-particles), the law of conservation of quasi-momentum, similar to that of linear momentum, holds: k i − k i = 2πb. i

i

Here k i and k i are the quasi-momenta of quasiparticles before and after a collision. To avoid ambiguity, the quasi-momenta of all colliding quasiparticles (before and after a collision) should be “located” in the same Brillouin zone. Therefore, if the number of colliding quasi-particles is not large, the vector of the reciprocal lattice, involved in the conservation law of quasi-momentum, does not exceed one or two elementary vectors of the reciprocal lattice. Collisions with b = 0 are referred to as normal collisions (emphasizing the satisfaction of the law of linear momentum con-

205

Schematic diagram of an Umklapp process.

servation), while collisions with b = 0 are called Umklapp processes (see Fig.). A periodic crystal lattice is a space where quasi-particles exist. The law of conservation of quasi-momentum is a corollary of the symmetry (periodicity) of this space, just as the law of conservation of linear momentum reﬂects the symmetry (uniformity) of empty space. Related to the uniformity of time is the law of conservation of quasi-particle energy in a crystal ε(ki ) = ε(ki ), i

i

where ε(ki ) and ε(ki ) are energies of quasi-

particles before and after a collision, respectively. Related to the law of conservation of angular momentum is the symmetry of the stress tensor in nonpolarized media. The essential information on the interaction of quasi-particles (as well as ordinary particles) can be obtained on the basis of a conservation law analysis of their kinematics. In particular, this is how selection rules are established that forbid processes where the conservation laws do not hold. The complexity of the dispersion laws of quasi-particles and the presence of Umklapp processes make the kinematics of quasi-particle collisions very complicated: mutual particle transformations, creation and annihilation, as well as breakup and fusion of particles, are possible. Even in the case of an elastic collision of quasi-particles (e.g., electron scattering by an impurity atom in a crystal), some unusual (for particles) situations are possible, e.g., the transition from one energy band (minimum) to another band (minimum), or

206

CONSTRUCTION MATERIALS Table 1. Criteria for materials of the ﬁrst wall of a tokamak Criteria I. Radiation damages and lifetime (a) swelling (b) blistering (c) surface atomizing II. Compatibility with cooler and tritium (a) Li (b) He (c) water (d) tritium III. Mechanical and thermal properties (a) yield point (b) ultimate stress limit σT (c) creep limit (d) thermal stress parameter M IV. Processibility and welding V. Developed industry and data base VI. Cost VII. Induced radioactivity

scattering when the particles scattered in a given direction have different quasi-momenta. CONSTRUCTION MATERIALS

Materials for production of engine parts, building constructions, etc., for which shape maintenance under mechanical forces is necessary. Metals and their alloys such as steel, natural and synthetic polymers, and ceramics are used as construction materials. Composite construction materials play a special role, and for usage in aviation and astronautics a reduction in weight without sacriﬁcing strength is important. The main quality factors of these materials are strength, elastic modulus, hardness, impact strength, and temperature dependence of physico-mechanical properties. CONSTRUCTION MATERIALS FOR THERMONUCLEAR REACTORS

Materials of thermonuclear reactor (TR) elements in contact with the plasma: ﬁrst wall, aperture, and divertor. The other parts of the reactor construction are exposed mainly to neutron irradiation so the choice of materials for them is less complicated. In the advanced TR design called the tokamak the main factors which affect the ﬁrst wall are: (1) neutron ﬂux with energy up

Materials Ti, V, Mo, stainless steel C, Nb, V, Ti, stainless steel V, Ti, Al, C Ti, V, Nb, Mo, stainless steel Stainless steel, Ti, Mo, Al, C Stainless steel, Al, Ti Mo, Al, stainless steel Mo, Nb, V, Ti, stainless steel Stainless steel, Ti, Al Mo, V, Ti, stainless steel Mo, Al, Nb, V Stainless steel, Al, Ti Stainless steel, Al, Ti, C C, Al, stainless steel, Ti V, C, Ti, Al

to 14 MeV and power up to 2.5 MW/m2 , (2) heat ﬂux with power up to 0.25 MW/m2 , (3) ﬂux of neutral atoms of hydrogen isotopes D and T generated at the ion recharge, j ∼ 1020 –1021 m−2 ·s−1 . The main factors which affect the aperture and divertor receiving plates are (1) ﬂow of D+ and T+ ions and heavy impurities with energies up to 20–50 eV, j ∼ 1023 m−2 ·s−1 , (2) heat ﬂux equal to 10–20 MW/m2 . In addition in a contingency the ﬁrst wall, aperture, and divertor should be able to sustain a discharge disruption and release of all the energy accumulated in the plasma (1–2 MJ/m2 ) during a time of 20 ms. For uncontrollable modes of TR operation the aperture and divertor can erode because of the development of unipolar arcs, i.e. electrical discharges between the plasma and plasma trap chamber. For design and economy reasons the ﬁrst wall cannot be changed, and should operate in an industrial reactor for ∼30 years. Aperture and divertor receiving plates are changeable. Table 1 cites main criteria for choice of materials for the ﬁrst wall of a tokamak listed according to their priority. The thermal stress parameter M M=

2σT k(1 − ν) , αE

CONTACT ANGLE

where k is the thermal conductivity, α is the thermal expansion, E is Young’s modulus, and ν is the Poisson ratio, characterizes the thermal stress from the temperature gradient: the greater the M value the greater is the allowable wall thickness. The tokamak operates in the pulsed mode, and the international reactor INTOR pulse lasts 200 s with a 20 s pause between. Thermal load cycling promotes the aging of materials. The most important features for the material choice for the aperture and divertor receiving plates are thermal and chemical properties, and surface erosion. For a hybrid reactor combining a thermonuclear and ﬁssion reactor which uses thermonuclear neutrons, construction materials will have less plasma applied loads because the high power of thermonuclear energy is not required, but the materials are subjected to radiation exposures typical of those from atomic ﬁssion reactors. CONSTRUCTION MATERIAL STRENGTH

The strength of construction materials or their models having design shapes and geometrical sizes typical of actual construction elements. In contrast to the material strength which is evaluated experimentally by testing relatively small material samples on devices of simpliﬁed shape, the constructional strength is evaluated by testing material samples with geometrical shapes and sizes that are typical of the majority of actual parts of engines or other devices. Values of constructional strength are much lower than those of material strength which is generally obtained for simpliﬁed laboratory samples. This difference arises mainly from the design shapes which often involve sharp transitions from one section size to another, the presence of holes which induce some stress concentration, and other factors. In addition, the surface quality of actual samples can differ considerably from the surface of laboratory ones because the handling technology of actual device production, as a rule, differs from the technology used for preparing simpliﬁed laboratory samples. The strength indices of actual samples are strongly inﬂuenced by their production technology, especially by welding which causes inhomogeneities in the material, and also the tangent stress due to so-called welding stresses.

207

Constructional strength is appreciably degraded by the decline of performance factors arising from exposure to repeatedly changing loads. There are always a number of factors under actual working conditions which cause the concentration of stress to be the main origin of the appearance of fatigue cracks on exposure to repeatedly changing stresses. CONSTRUCTION PLASTICS

Plastics (see Polymeric materials) designed for the production of parts and components capable of keeping their shape during exposure to mechanical loads. Polyoleﬁnes, polyformaldehydes, polyamides, ﬂuoroplasts, polyarylates, etc. are used in various industries as constructional plastics. The main processing methods for converting these plastics into components are pressure die casting, hydroextrusion, and pressing. In most cases constructional plastics are multicomponent systems: antioxidants, lighting stabilizing agents, plasticizing agents, oilers, bulking agents, etc., which are loaded as additional binders that impart speciﬁc properties (e.g., ber glass, carbon, boron nitride, ﬁre-retardant additives, etc.). CONTACT ANGLE

Angle between surfaces of a ﬂuid and a solid body (or another ﬂuid) in contact. The contact angle θ is counted from the ﬂuid. The equilibrium contact angle is referred to as the edge angle and is denoted by θ0 . During contact formation the angle varies from θ = π up to θ ≈ θ0 during 0.02–0.03 s. On rough solid surfaces the contact angle usually decreases, so that for θ < π/2, cos θ = γ cos θ0 , where γ is the surface roughness coefﬁcient. The contact angles for ﬂuid inﬂow on a substrate θin , and for outﬂow θex , differ from θ0 . This is caused by the roughness and heterogeneity of the actual surface. For substrate backings with a high surface energy the property of “autophobia” is possible in contact with polar ﬂuids: the ﬂuids on the substrate generate adsorption ﬁlms on which they form a contact angle θ > 0. It is known that θin > θ0 > θex , and this effect is referred to as wetting hysteresis. With increasing

208

CONTACT CORROSION

temperature θin → θ0 and θex → θ0 , so the hysteresis decreases (see Wetting). CONTACT CORROSION, galvanic corrosion A type of electrochemical local corrosion re-

sulting from the contact of two or more metallic materials with different initial corrosion potentials, situated in a conductive corrosion environment. The contact corrosion intensity is determined by a polarization cathode and anode resistance, the ratio of their dimensions, and decreases with increased distance from the contact point. The metal quantity being dissolved because of contact corrosion is equivalent to the current. Methods for protecting against contact corrosion consist of sensible equipment designing, eliminating or isolating contacts of metals having much different corrosion potentials, using protectors, etc. CONTACT POTENTIAL DIFFERENCE

Difference of electric potentials between surfaces of conductors brought into contact at thermodynamic equilibrium. It is deﬁned by the difference in the work functions of the media in contact divided by the electron charge. The contact potential difference arises from the requirement of electrochemical potential equality for media in contact; it is established because of electron exchange between the conductors. Thus the surfaces of both media become charged: negative for the conductor with the greater work function, and positive for the other. The width of the boundary (contact) layer in which the electric ﬁeld differs from zero is deﬁned by the shielding distance in the conductor, with values 10−10 –10−9 m for metals and up to 10−6 m for semiconductors. The potential difference can reach several volts, and depends on the physico-chemical condition of the boundary region. In multiple layer heterophase structures representing a chain of conductor contacts the overall potential difference does not depend on the intermediate links, but equals the potential difference of the extreme outer conductors. This potential difference is important for the formation of electrovacuum devices and solid contact structures: semiconductor junctions, heterogeneous structures, metal–semiconductor junctions, etc.

CONTACT PROBLEM OF ELASTICITY THEORY Determination of the strain and stress distrib-

ution in a system of solid bodies having a general contact surface. For the case of two elastic bodies in three-dimensional space this problem was set up and solved ﬁrst by H. Hertz (1882) by considering that the contact area consists of small, strain-free surfaces around the contact point referred to as second-order surfaces. With the help of an electrostatic analogy he determined the pressure function at the contact point, and derived explicit formulae relating the magnitude of the impression h, the impressing force F , and the main radii of curvature of strain-free surfaces at the contact point, from which a relationship of the type h = const · F 2/3 followed. Among contact problems of the theory of elasticity are stamp problems in which one of contacting bodies is an elastic halfplane, and the other is an perfectly rigid body impressed into the halfplane by ﬁxed forces. In the simplest case of a ﬂat die uniformly pressed onto the boundary of a half-plane on the segment (−a, a) of the Ox axis the contact pressure distribution P (x) is determined by the formula P (x) = F /[π(a 2 − x 2 )1/2 ] where F is the pressing force. One approach to solving such a problem involves reducing it to a boundary value problem of the theory of analytical functions. CONTACT STRESSES, mechanical

Stresses which appear at mechanically interacting solid deformable bodies, or around them (e.g., at the compression of bodies in contact). Knowledge of contact stresses is important for the strength calculation of bearings, gear and worm transmissions, ball and cylinder compactors, colliding bodies, etc. The contact surface size is often small in comparison with the body dimensions, with the contact stresses rapidly decreasing with distance from the initial contact point. The stress distribution at the contact area and in its neighborhood is nonuniform, and the peak shearing stresses which characterize the strength of compressed bodies can appear at a particular distance from the contact point. In Fig., the upper part shows two spheres in contact, subject to the compression force P , with A indicating the point of peak stress. The lower part shows how the stress p in the interface decreases with the radial distance r

CONTINUUM MECHANICS

209

a Euclidean space, however, any part of such a sphere is homomorphic to a certain region of Rn . Lie groups are among the most important transformation groups used in physics. For example, various conservation laws are related to such groups. The Lie groups most often found in physics are the orthogonal groups O(n) and the unitary groups U (n) of real- and complex-valued n × n matrices, which preserve their scalar product in the real, Rn , and complex, Cn , Euclidean spaces, respectively. Their subgroups consisting of matrices with a unit determinant (det = +1) are called special orthogonal groups and special unitary groups, denoted by SO(n) and SU(n), respectively. Spherical harmonics transform by SO(n), and spinors (S = 1/2) by SU(2). CONTINUUM INTEGRAL See Path integral. CONTINUUM MECHANICS, mechanics of continua

Upper part: two spheres in contact subject to the compression force P , with the point of peak stress designated by A. The region of contact has the radius a. Lower part: the stress p variation with the radial distance r from its peak value p0 in the center.

from its peak value p0 in the center of the contact area. See also Contact problem of elasticity theory. CONTINUOUS SYMMETRY TRANSFORMATION GROUPS, Lie groups (S. Lie)

Transformation groups with continuous symmetry. Inﬁnite groups in which a ﬁnite number of parameters, n, corresponds to each element of the group. Here, the group operations (i.e. mappings (g, h) → gh and g → g −1 for elements g and h of a group G) must be continuous and inﬁnitely differentiable functions in the parameter space. A number n is called the group dimensionality. In general, the n-dimensional Lie group is a topological space (differentiable manifold), the neighborhood of each of its points being homomorphic to a certain region in Euclidean space Rn . For example, an n-dimensional sphere Sn is not

Branch of mechanics devoted to describing the properties and movements of matter (solids, liquids, gases, plasma, etc.) in the continuum approximation. This approximation involves long wave length vibrations (λ lattice constant) with small propagation constants k = 2π/λ. The mechanics of continua may be divided into the mechanics of deformable solids (including elasticity theory, plasticity theory, theory of failure, etc.), hydrodynamics, gas dynamics, etc. The continuum approximation applies to any dynamic system that consists of a large number of particles that may be considered as a homogeneous medium. This description is predicated on introducing physically inﬁnitesimal volumes, whose size (l mic ) far exceeds characteristic distances between particles (l part ). Averaging microscopic mechanical characteristics of the system (forces, coordinates, momenta of particles, energy, etc.) yields macroscopic quantities (density, velocity ﬁeld) that have a continuous distribution in space. The equations of motion of particles undergo a similar averaging; to obtain closed form equations for the above macroscopic quantities. To accomplish this it is necessary, as a rule, to perform a certain “uncoupling” of cross-terms of dynamic equations. The latter procedure imposes a limitation on l mic ,

210

CONTINUUM MECHANICS

i.e. l mic l mac , where l mac is the characteristic length of variations of averaged macroscopic quantities. One can obtain in this manner, e.g., hydrodynamic equations from quantum equations of motion of the density matrix, or equations of elasticity theory from classical equations of motion of crystal ions. Thus the validity criterion for the present description of a dynamical system of a large number of particles is of a self-consistent nature, and is stated in the form of an inequality l part l mic l mac . This criterion corresponds to sufﬁciently homogeneous systems (gases, liquids). In the case of inhomogeneous systems that contain many (macroscopic) structural elements this description may prove to be too detailed, and it may be necessary to perform a second averaging of macroscopic equations of motion over volumes of a larger characteristic size l that satisﬁes the . Here, l inequality l str l lm str is the characteristic size of structural elements or the mean is the characteristic distance between them, and lm length of variations of doubly averaged quantities. Typical examples are the averaged description of the motion of multiphase media with a heavy mixing of phases (i.e., attenuation of sound in solids with many pores, or the elastic properties of a composite material), plastic ﬂow of solids under conditions of a high density of dislocations and dispersed particles, and the possible propagation of a main crack in a material with a number of microcracks and cavities in the zone of failure. Two equivalent methods are used for describing the motion of macroscopic particles of continuous media. The Lagrange method involves tracking the location of a particle r = r(a, t) at every instant of time t ; vector a speciﬁes the particle, and is usually taken to be the particle location at the initial instant of time t0 . The Euler method involves tracking the velocities, accelerations, etc. of various particles that pass through a certain point r of the space. Ordinarily the Eulerian description is used when the mechanical state of the medium is characterized by ﬁelds of various types: displacement ﬁeld u(r, t), velocity ﬁeld v(r, t), density ﬁeld ρ(r, t), etc. The ﬁelds usually satisfy second-order partial differential equations (Navier–Stokes equations of hydrodynamics, equations of elasticity theory, etc.). Along with u and v, these equations involve the force characteristics of the medium, described most often by

the ﬁeld of the stress tensor σik (r, t). Evaluating the system of equations of the mechanics of continua requires specifying the constitutive relations (rheological equations) that establish a link between σik and u, v. In the case of a solid under smooth and rather small strain, this link may be considered linear and local (i.e. σik (r, t) depending on the values of u, v, taken at the same point r and at the same instant of time t ). More complicated relationships between σik and u, v are also possible (linear, nonlocal, with allowance for the history of deformation of the medium), represented by complicated functions σik = fik (u, v) or by functionals σik = &{u(r, t), v(r, t)}. For instance, we have for a linear nonlocal medium Alm σik (r, t) = ik (r, t; r , t )ulm (r , t ) dr dt . Equations of continuum mechanics in the linear local approximation often proceed from general considerations (law of conservation of particle number, symmetry conditions, etc.). They contain a number of unknown coefﬁcients (elastic moduli, coefﬁcient of viscosity, etc.) that should be determined experimentally or calculated from a microscopic theory. The above procedure for obtaining macroscopic equations from microscopic ones involves not only purely spatial averaging, but also statistical averaging (for quantum dynamic systems both kinds of averaging are performed simultaneously through the density matrix). Statistical averaging may fail to produce closed mechanical equations, since the continuum equations may contain thermodynamic and chemical quantities (temperature, concentration, chemical potentials, etc.) along with parameters characterizing internal degrees of freedom of microparticles or other subsystems of the body (electric, magnetic, and others). In this case, the mechanical problem should be solved together with the thermal, chemical, etc. ones by adding equations of thermal conductivity, diffusion, etc. to continuum mechanics equations. Typical examples are diffusive-viscous creep of polycrystals (see Diffusion mechanism of crystal creep), dynamics of ferroelectrics and ferromagnets, and propagation of shock waves in crystals. Besides that, empirical or calculated relationships may be available, which describe the

COOLING DUCT

dependence of mechanical parameters (e.g., elastic constants) on temperature, concentration, magnetization, etc. The most consistent description of related mechanical, thermal, electrical, and magnetic processes can be made within the framework of the thermodynamics of irreversible processes, which includes much of continuum mechanics as a special case. In certain situations, however, one can conﬁne oneself to the solution of a purely mechanical problem. For instance, in a static state during a very slow deformation of a solid, the temperature has time to equilibrate and the deformation process is described by equations of elasticity theory with isothermal elasticity moduli. Also, under very rapid deformation (e.g., propagation of high frequency sound), heat transport between neighboring parts of a body does not take place, and the process is described by the same equations, but with adiabatic elastic moduli. CONTINUUM THEORY OF DEFECTS Theory of defects in a broad sense based on

the continuum approximation in analysis. From a more specialized viewpoint the continuum approach to defects is founded on the assumption that they ﬁll the physical space of the crystal. The subjects of this analysis are usually dislocations, disclinations, dispyrations, and planar defects, although the methodology can be extended to other problems which are not closely related to the presence of defects: e.g., this theory is used for the calculating thermal stresses, electrostrictive or magnetostrictive mechanical effects (see Electrostriction, Magnetostriction), elasto-plastic ﬁelds generated by phase transitions or twinning of crystals, etc. This continuum theory is constructed on rather general physico-mechanical principles. It includes the determination of the tensor of densities of defects, the balance conditions for these densities, and the continuity condition (existence of solutions). In this theory the connection between defect motion and the plastic ﬁelds generated by this motion (see Plastic deformation) is analyzed. The forces acting in this process and other factors are evaluated. The system of equations in the continuum theory involves a fundamental relation that connects the mobility of defects and the forces acting on them. This fundamental equation is considered to be known because it cannot be

211

derived, apparently, within the framework of the continuum approximation. CONTRACTION, TRANSVERSE

See Transverse contraction. CONVOLUTION OF LINE SHAPE

See Line shape convolution. COOLING AGENT, refrigerant

A material (working medium) used to cool a substance (cooling agent) or maintain it at a low temperature (cryo-reservoir). The most widely used refrigerants are liquids and gases with low condensation and crystallization temperatures (3 He, 4 He, H2 , Ne, N2 , CO2 /acetone, etc.), paramagnetic salts (magnesium cerium nitrate Ce3 Mg3 (NO3 )12 ·24H2 O, ferric chromium alum and ferric aluminum alum), van Vleck paramagnets (PrNi5 , PrPt5 , PrTl5 , PtCu6 , etc.), metals with paramagnetic nuclei (Cu, Ag, In, etc.). COOLING DUCT

A heat exchanging device to provide the thermal connection of an object being cooled with a cooling agent (refrigerant), or with a cryostat (low-temperature reservoir). In the simplest case a cooling duct is a rod (tube, stripe, etc.) of a material with good thermal conductivity, which provides a reliable thermal connection with the parts of an installation containing the object being cooled, as well as the cooling agent, or the low temperature reservoir. Often (especially at low temperatures) the cooling duct is in the form of a large number of thin wires (usually made of copper) which improves the heat transfer efﬁciency by increasing the contact area. To arrange for the adjustment of the temperature the cooling duct can be provided with a heater, and when it is necessary to rapidly change the thermal connection then heat switches are used. The associated properties of a thermal switch and a cooling duct are combined in a thermosiphon, which is an hermetically sealed tube ﬁlled with a gas under pressure, providing for its liquefaction in the desired temperature range.

212

COOPERATIVE LUMINESCENCE

Cooperative luminescence.

COOPERATIVE LUMINESCENCE Luminescence caused by radiative transitions

from excited states in crystals that result from the delocalization of energy from individual excited states (e.g., photoexcited states of impurity centers); it is a special case of anti-Stokes luminescence. Cooperative luminescence violates the Stokes’ rule and Vavilov law. The phenomenon was discovered by C.A. Parker (1962) and F. Muel (1962) in dye solutions. In the solid state it was observed by P.P. Feoﬁlov, V.V. Ovsyankin (1966) and separately by F. Auzele (1966) in crystals activated with rare-earth ions, and in broad-band semiconductors with an adsorbed dye. An example of the mechanism of cooperative luminescence is the absorption of light by local crystal centers (transitions 1 → 2 and 1 → 2 ), the addition of photoexcitation energy to induce the transition from one of these excited states to the 3 level, followed by the subsequent radiative transition 3 → 1 (Fig. (a)). This luminescence process can also occur through excitation energy transport from two local centers (2 and 2 levels) to a third (level 2 ), with the subsequent radiative deexcitation of the latter (2 → 1 ) (Fig. (b)). COOPER EFFECT (L. Cooper, 1956)

Instability of the ground state of a fermion system with respect to the spontaneous formation of bound pairs of fermions with antiparallel momenta and spins (see Cooper pairs), provided that an arbitrarily weak attraction V0 < 0 exists between these particles in a narrow energy band near the Fermi surface. The binding energy of a selected pair of fermions (lowering of its energy with respect to the Fermi level, EF ) is equal to

E = ω0 e−2/g , where g = N(EF )V0 is the dimensionless coupling constant, N(EF ) is the density of states at the Fermi surface, and ω0 EF . In momentum space the Cooper effect is similar to the quantum-mechanical formation of a bound state that develops when a particle of mass m moves in a two-dimensional rectangular potential well of depth U0 and width a. Within the limit of weak coupling (shallow and narrow well) the energy of the lowest level depends exponentially on the interaction constant: E0 ∝ U0 e−1/g0 , where g0 ∝ U0 a 2 m/2 . While treating the problem initially and selecting an isolated pair of fermions (i.e. electrons) from the Fermi sea, L. Cooper ignored the principle of particle identity, but took into account the Pauli principle. A more systematic self-consistent treatment of the problem was provided by J. Bardeen, L. Cooper and J. Schrieffer (1957) (see Bardeen–Cooper–Schrieffer theory). COOPER PAIR, KINETIC DECOUPLING See Kinetic decoupling of Cooper pairs. COOPER PAIRS

Correlated bound states of fermion pairs (electrons, sometimes holes) with opposite quasi-momenta and antiparallel (singlet) or parallel (triplet) spins, that form due to an attractive interaction (see Cooper effect). Such an attraction in metals (semimetals, doped semiconductors etc.) between conduction electrons (holes) near the Fermi surface at low temperatures can be produced by the exchange of virtual phonons. For a strong enough electron–phonon interaction the attraction may override the screened Coulomb repulsion. The Cooper pairs formed by this attraction have the binding energy 2Δ EF (Δ is the energy gap, EF is the Fermi level), and are characterized by a correlation radius larger than the average electron-to-electron distance r = 10−9 m. This is the so-called coherence length ξ = 10−8 m, so that the wave functions of Cooper pairs strongly overlap. As a result a coherent condensate of Cooper pairs forms within the volume of the crystal (see Bose condensate) that is described by a complex wave function ψ = |ψ|eiθ (the order parameter) with a phase θ that is, generally, coordinate dependent. Since the spin of a Cooper pair

COORDINATION SPHERE

is an integer (0 or 1) it is a Boson particle, and a Bose–Einstein condensation called a Cooper pair condensate can form in which all of the pairs are in the same quantum-mechanical ground state. However, Cooper pairs have been called “bad” bosons + + a−p,−σ and annihisince their creation Bp+ = apσ lation Bp = a−p,−σ apσ operators are more com+ plicated than the usual creation apσ (annihilation apσ ) operators of a fermion with momentum p and spin s = ±1/2 (see Second quantization). Cooper pairs have the more complex commmutator relations Bp Bp+ − Bp+ Bp = (1 − npσ − n−p,−σ )δpp , instead of the usual Bose operator commutation rules. Here δpp is the Kronecker symbol and + apσ is the number operator, which npσ = apσ is 1 for an occupied state and 0 for an unoccupied one. The Cooper pair condensate state is separated by a gap of 2Δ from excited states (excitations above and below the Fermi surface), the latter having a continuous spectrum εp = ±(Δ2 + vF2 (pF − p)2 )1/2 that satisﬁes the Landau super uidity criterion (vF and pF are the Fermi velocity and Fermi momentum, respectively). Thus, the formation of Cooper pairs in a charged electron Fermi liquid (or Fermi gas) in metals results in superconductivity, while in a neutral Fermi system (3 He, neutron matter) a process involving rotons results in the related phenomenon of super uidity (see Super uid phases of 3 He). COORDINATION COMPOUNDS

These are compounds of complex composition in which a central atom or ion (complexing agent) has molecules and ions called ligands bound to it by donor–acceptor bonds (see Donor–acceptor pairs). The central metal atom or ion is generally a transition metal with electron-acceptor properties. Ligands representing electron donors can be neutral molecules (H2 O, NH3 , CO, etc.) or − anions (C2 O2− 4 , CN , etc.). The central atom together with its ligands form the “complex” or inner coordination sphere of complex compounds, and examples are [Fe(CN)6 ]3− , [Co(NH3 )6 ]3+ and [Pt(NH3 )2 Cl2 ]. The inner sphere is usually enclosed in square brackets. The complex can be neutral or charged, in the latter case it is a cation

213

(+) or anion (−), and counterions (monatomic or complex) comprise the outer coordination sphere. To separate the complex ion from its component + ions such as SO2− 4 or NH4 one can assume that the reaction of complex formation from the central atom (ion) and ligands can occur under normal chemical conditions, and that the central ion is capable of existing independently in solution in a solvated form. This limitation is of a conditional character since there is no essential difference be− tween such ions and, for example, PF− 6 and VF6 in their chemical bond nature, and the majority of their physico-chemical characteristics. Each ligand is attached to the central atom through one, two, or several atoms occupying, respectively, one (monodentate ligand), two (bidentate ligand) or several (polydentate ligand) coordination sites. The total number of coordination sites in a complex is its coordination number, and it is determined by the central atom oxidation state and by the nature of the ligand. Complexes with coordination number six and octahedral symmetry are the most widespread ([PtCl6 ]2− , [Ru(NH3 )6 ]2+ ); others are commonly four-fold coordinated with square planar ([PtCl4 ]2− ) or tetrahedral ([CoCl4 ]2− ) symmetry. Coordination polyhedra can be distorted through ligand inequivalence, electronic effects (see Jahn–Teller effect) or crystal lattice inﬂuences. COORDINATION SPHERE

A sphere centered at a particular atomic site with surrounding atoms of the crystal located on its surface. Coordination spheres are numbered in the ascending order of their radii: the ﬁrst (closest), then the second, and so on. The ﬁrst sphere contains the z nearest neighbors of the given atom, where the coordination number z is is a measure of the packing density of the atoms; the most loosely packed semiconductor structure is the diamond type (Si, Ge) with z = 4, in NaCl type ionic crystals z = 6, in BCC metals and those with the ﬂuorite structure (ceramics) z = 8, in FCC and HCP metals z = 12. In ideal crystals the coordination sphere radii coincide with peak positions of the radial distribution function (RDF), with the number of atoms in the nth sphere proportional to 4πrn2 Sn , where Sn is the space under the nth RDF surface. Using this correspondence, the coordination sphere concept can be extended to liquids and

214

COPPER

amorphous solids (see Amorphous state), understanding as the nth coordination sphere the spherical layer with atom positions within the range rn of radius values rn corresponding to the magnitude of nth RDF peak, and considering the number of atoms in the nth sphere as 4πrn2 Sn ρ, where ρ is the average atom density. For an amorphous solid, with increasing r the RDF peaks rapidly broaden and become ﬂattened, so the coordination sphere concept is used only for small n (usually n = 1–3). Thus, in virtue of the statistical nature of the RDF the number of atoms in the sphere (the coordination number) can be nonintegral. The coordination sphere concept is useful in the analysis of structures with short-range order (see Long-range and short-range order), for self-ordered alloys, for the approximate construction of a crystal potential for band structure calculations, and so on. COPPER (Lat. cuprum ), Cu

Chemical element of Group IB of the periodic table with atomic number 29 and atomic weight 63.546. Stable isotopes 63 Cu (69.1%) and 65 Cu (30.9%). Nine radioactive isotopes are known. Outer shell electronic conﬁguration 3d 10 4s 1 . Successive ionization energies (eV): 7.72, 20.29, 36.83. Atomic radius is 0.127 nm. Ionic radii are (nm): Cu+ 0.096, Cu2+ 0.072. Covalent radius 0.117 nm. Oxidation states +1, +2, more rarely +3. Electronegativity is 1.75. Copper is a red-tinted metal of face-centered ¯ (O 5 ); a = cubic structure, space group F m3m h 0.361479 nm. Density is 8.932 g/cm3 ; Tmelting = 1356 K, Tboiling = 2843 K, heat of melting 13.0 kJ/mole, heat of sublimation 340 kJ/mole, heat of evaporation 307 kJ/mole (under standard conditions). Speciﬁc heat is 390 J·kg−1 ·K−1 at 298 K. Debye temperature is 339 K; linear thermal expansion coefﬁcient 16.8·10−8 K−1 . Coefﬁcient of thermal conductivity is 385–402 W·m−1 ·K−1 (at 273 K) and 5 W·m−1 ·K−1 (at 20 K). Adiabatic elastic moduli of crystal: c11 = 168.8, c12 = 121.8, c44 = 75.5 GPa at 298 K. Young’s modulus is 110–145 GPa, shear modulus is 42–55 GPa, Poisson ratio is ≈0.33. Rupture strength is ≈230 MPa, relative elongation 60%. Brinell hardness is 35 HB (at 293 K). Coefﬁcient of selfdiffusion is 9.1·10−14 m2 /s (at 1233 K). Lowtemperature linear electronic heat capacity coefﬁcient 0.687–0.695 mJ·mole−1 ·K−2 . Electric

resistivity is 15.5 n·m. Electric resistance temperature coefﬁcient is 440·10−5 K−1 (at 273– 373 K). Hall constant is −5.2·10−11 m3 /C. Absolute thermal electromotive force coefﬁcient +1.7·10−6 V/K. Reﬂection factor for 5 μm optical wave is 98.9%. Work function of a copper polycrystal is 4.4 eV. Copper is diamagnetic with magnetic susceptibility (5.4–10)·10−6 CGS units. Ion plasma frequency is 7.655 THz. About 50% of copper produced is used in the electrical power industry, and over 30% is used for copper alloys. It is widely used for chemical equipment. COPPER ALLOYS Copper forms the following systems with other elements: (a) inﬁnite solubility in solid and liquid

states: with Ni, Rh, Pt, Pd, Mn, Au; (b) inﬁnite solubility in liquid and limited solubility in solid state: with Li, B, Ag and Bi; (c) peritectic type of interaction (see Peritectic alloys): with Ir, Nb, Co, Fe; (d) limited solubility in liquid and solid phases: with Pb, Tl, Cr, V); (e) intermediate compounds with many elements (for dissimilar electrochemical properties Cu forms chemical compounds; for the same properties, an electron compound is formed). Cu dissolves up to 31.9 Zn, 20 Li, 16.6 Be, 16.4 Ga, 15.8 Al, 12 Ge, 11.15 Si, 10 In, 8 Ir, 8 Ti, 8 Sb, 7.7 Sn, 7 Mg, 6.85 As, 4.5 Fe, 3.4 P, 2.1 Cd (molar content, %). Some copper alloys have special names: bronzes (with Al, Sn and some others), brasses (with Zn), German silver (with Ni). On addition of Zn, Sn or Al to Cu, α-solid solutions appear ﬁrst; then, as the concentration increases, β-, γ -, δ-phases appear, and so on. All industrial brasses and bronzes are of two types differing in structure and properties: single-phase α-alloys (plastic, easily deformable, strength and hardness slightly exceeding those of copper) and two-phase alloys (α-solid solution + another phase). The latter exhibit higher strength and hardness but lower plasticity. Of practical use are brasses that contain up to 43% Zn, tin bronzes with up to 22% Sn, aluminum bronzes that contain up to 11% Al. Tin bronzes exhibit enhanced strength, hardness, corrosion resistance (α-bronzes that contain up to 7– 8% Sn). Aluminum bronzes are stronger and more plastic, corrosion- and wear-resistant; two-phase alloys are commonly used (≈ 10% Al). Quenching and tempering (because of phase transitions

CORRELATION ENERGY

in the solid state) may change their properties essentially. Silicon bronzes exhibit less speciﬁc weight and high mechanical properties. If silicon content is 2–5%, they are mostly single phase and often used with Mn, Fe, Zn additions. Beryllium bronze (2–3% Be) exhibits high elasticity, corrosion resistance. In cadmium bronze Cd improves the strength of Cu. Lead bronze separates into layers already in the liquid phase; at Pb content of 20–30%, it is used as a bearing alloy. Cu forms the following compounds with Ni: copper– nickel (32% Ni), constantan (40–45% Ni) that exhibits high electrical resistance, bullet German silver (20% Ni). Single phase alloys with Mn possess enhanced electrical resistance: manganin (12% Mn + (2–4)% Ni) and double manganin (20% Mn + 5% Al) with electrical resistance twice that of manganin. CORBINO DISK (O.M. Corbino, 1911)

A metal or semiconductor disk with a hole in the center, with a contact located on the inner wall of the hole, and another at the periphery. It is used for investigating galvanomagnetic effects. The plane of the disk is normal to an external magnetic ﬁeld B. When electric current ﬂows between the contacts, due to the sample axial symmetry the electric ﬁeld has only a radial component and the Hall ﬁeld is absent. As a result, there is no (partial) compensation for the curvature of charge carrier paths in the magnetic ﬁeld by the Hall ﬁeld, and the relative resistance R/R in the magnetic ﬁeld appears to be much greater than the magnetoresistance value ρ/ρ0 (ρ0 is the resistance with the ﬁeld absent, and ρ is the change brought about by the ﬁeld) measured in a long (thread-like) sample. In n-InSb at 300 K in a ﬁeld B = 1 T,

R/R = 17.7, and ρ/ρ0 = 0.48. These values are connected by the relationship

R

ρ (μH B/c)2 = + R0 ρ0 1 + ( ρ/ρ0 ) (μH is the Hall mobility of charge carriers) from which it follows that when B increases the ratio

R/R does not tend to saturation. Therefore, the Corbino disk is utilized in devices for strong magnetic ﬁeld measurement (see Magnetometry).

215

CORRELATION in alloys

The interconnections in the equilibrium distribution of alloy component atoms on crystal lattice sites. They depend on the differences in the interaction energies of different atoms since each atom tends to surround itself by atoms of another type in ordered alloys, or by the same atoms in dissociating alloys (see Alloy ordering, Alloy decomposition). Quantitative measures of this correlation are correlation parameters, or short-range order parameters. The latter characterize mainly the extent of the formation of pairs of dissimilar atoms, or pairs of identical ones. CORRELATION ENERGY

The difference between the ground state energy of an interacting particle system and the minimum energy of the system determined by a selfconsistent eld method. The correlation energy concept is most often used for the description of an electron gas. For the self-consistent Hartree–Fock method the correlation energy is the true energy minus the kinetic, electrostatic and exchange energies. In this case the correlation energy is related to the decrease in energy due to the vanishing of the probability density for the presence of two electrons at the same point because of the singularity of the Coulomb interaction. A rigorous calculation of the correlation energy always represents a complicated problem, especially when dealing with a crystal or a polyatomic molecule. In such cases the wave function is represented by a superposition of antisymmetrized products of one-particle states (in Hartree–Fock theory only one such term is retained), see Con guration interaction, or the wave function is formed on the basis of two-, three-, and so on molecular orbitals (e.g., geminals). The correlation energy of a homogeneous electron gas is the best studied. Here the energy, according to Hartree–Fock theory, corresponds to the ﬁrst order of the perturbation theory of the interelectronic interaction, and the correlation energy is the sum of the remaining terms of a series, each term of which diverges. Several ways are known for summing these series that result in the expansion of the one electron correlation energy 22 εcorr = 2(1 − ln 2) ln rs − 0.096 + Ars ln rs me4 + Brs + · · · ,

216

CORRELATION ENERGY OF A CENTER

where rs = [3n/(4π)]1/3 is the average distance between electrons in Bohr radii [2 /(me2 )], and n is the number of electrons per unit volume. This expansion in powers of rs cannot be rigorously justiﬁed for real valence electron densities for which 1.5 < rs < 6. Nevertheless, the known results for the correlation energy are in good agreement with those obtained with the aid of the variational principle, that are not dependent on the smallness of rs . The correlation energy of inhomogeneous systems is more often calculated within the framework of density functional theory (see Density functional theory) using the approximation of local homogeneity. This gives Ecorr = εcorr n(r) n(r) d3 r. The exchange interaction energy is not always separated from the correlation energy, and then one speaks about an exchange-correlation energy. CORRELATION ENERGY OF A CENTER

The difference U between the energies E1 and E2 in the sequential trapping of the ﬁrst (1) and the second (2) electron on alternative levels of a local electronic center (see Local electronic levels) in a non-metallic crystal. Because of the mutual repulsion of electrons the relation U = E1 − E2 > 0 (positive correlation energy) is the usual one. The energy level positions and the charge states of the center for U > 0 are shown in Fig. (a, b) for a doubly-charged and an amphoteric center, respectively. The deformation of the atomic environment of the center caused by the strong interaction of the electrons with the atomic subsystem can give rise to a signiﬁcant increase of the potential well and the binding energy of the second electron on the center. In this case the relation U < 0 (negative correlation energy) becomes possible. Centers with a negative correlation energy are ﬁlled pairwise by electrons under the condition of thermodynamic equilibrium. In particular, if an amphoteric center concentration with U < 0 dominates, then one half of the centers are ﬁlled with pairs of electrons and have a negative charge, and the other half have a positive charge. The Fermi level EF thus is located in the middle between the donor and acceptor levels (Fig. (c)), and does not vary with a change in the concentration of the centers (socalled pinning). The amphoteric interstitial boron

Donor (D) and acceptor (A) energy levels between the top of the valence band (Ev ) and the bottom of the conduction band (Ec ) for positive (U > 0) and negative (U < 0) correlation energies, where EF is the Fermi energy.

atom in silicon is an example of a center with a negative correlation energy, another example is the Si V vacancy in silicon, where U < 0 for the trapping of the second electron on V − , and for the trapping of the second hole on V + . CORRELATION FUNCTION

The average of the product of several variables or functions corresponding to different points in space–time. Correlation functions describe the correlation of dynamic variable values. A correlation function or correlator of nth order is the quantity ξ1 (X1 )ξ2 (X2 ) . . . ξn (Xn ), where Xi = (xi , yi , zi , ti ), x, y, z are the space coordinates, t is the time; ξi is a dynamic variable or function, and stands for a certain averaging. In classical physics ξ(X) represents a random (often complex) ﬁeld, and the averaging is carried out over all possible ﬁelds under consideration. In the particular case when ξi depends only on time ξi = ξi (t) represents a random quantity, and the averaging is carried out over time. In quantum physics the ξi (Xi ) represent Heisenberg operators describing quantum ﬁelds, and the averaging is carried out over some state of the ﬁelds speciﬁed by the statistical operator (density matrix) ρ: ξ1 (X1 ) . . . ξn (Xn ) = Tr{ρξ1 (X1 ) . . . ξn (Xn )}. The Heisenberg operators can depend only on time, thus ξ1 (t1 ) . . . ξn (tn ) = Tr{ρξ1 (t1 ) . . . ξn (tn )}. An important case arises when the ξi represent operators for the creation

CORRELATION TIME

or annihilation of ﬁeld quanta (see Second quantization), or of particles (quasi-particles), or the quantum system as a whole in a certain state: ξi = ai+ or ai . In solid state physics these are creation and annihilation operators of electrons (holes), excitons, phonons, magnons, photons, or states of impurity centers (see Impurity atoms). In solid state quantum theory pair correlations ξ1 (t1 )ξ2 (t2 ), or second-order correlation functions ξ1 (X1 )ξ2 (X2 ), are the most widely used. When considering the pair correlator it is convenient to use average and difference times: t = (t1 + t2 )/2, τ = t1 − t2 , hence ξ1 (t1 )ξ2 (t2 ) = f (τ, t). Of fundamental importance is the spectral representation f (ω, t) = eiωτ f (τ, t) dτ which deﬁnes the system spectral characteristics. In the stationary case the dependence on t is absent. The pairwise temporal correlator f = a + (t1 )a(t2 ) in its spectral representation describes, through the frequency or the energy E = ω, the occupation of the state to which the operators a + , a are related. To evaluate the correlation function it is usually more effective to use the related Green’s functions. CORRELATION FUNCTION OF RANDOM FIELD

A statistical characteristic of a random ﬁeld (see Random potential) in a disordered system deﬁned by the equality ψn (r 1 , . . . , r n ) = V (r 1 ) . . . V (r n ), where n 2 is the order of these functions. Here 1 . . . n means averaging over the random ﬁeld Vr , and the origin of the energy scale is selected so that V = 0. Most widely used is the pair correlation function of a random ﬁeld ψ2 in terms of which many experimentally measured quantities can be expressed, such as the square of a random ﬁeld ﬂuctuation V 2 (r). In the Gaussian random ﬁeld case all functions ψn (n 3) are expressed in terms of ψ2 . In a macroscopically homogeneous disordered system the functions ψn (r 1 , . . . , r n ) depend only on (n − 1) differences r 1 − r n , r 2 − r n , . . .; and in particular, ψ2 (r 1 , r 2 ) = ψ2 (r 1 − r 2 ). An important property of random ﬁelds in real systems is the attenuation of correlations in systems at inﬁnity. With the distancing of the points r 1 and r 2 from each other the correlation of

217

the quantities V (r 1 ) and V (r 2 ) decreases. This provides an opportunity for the factorization of the average of the types V (R 1 ) . . . V (R n )V (r 1 ) . . . V (r m ) = ψm (r 1 , . . . , r m )ψn (r 1 , . . . , r n ), if R i = r i + α and |α| → ∞. In particular, ψ2 (r) → 0 as |r| → ∞. The distance |r 1 − r 2 | at which the pair correlation function ψ2 (r 1 , r 2 ) becomes and remains a negligible quantity is called the correlation radius or correlation length. This radius is an important characteristic length scale of a random ﬁeld, which determines the behavior of macroscopic quantities that depend on the ﬁeld. See Correlation length. CORRELATION LENGTH, correlation radius

The characteristic dimension of the region within which correlation between physical variables is appreciable. At distances exceeding the correlation radius these variables become statistically independent of each other, and their correlation function becomes equal to the product of their averages. Consider, e.g., a ferromagnet that is far from its critical point (transition temperature). The correlation radius is of the order of an interatomic distance. Thermal motions and quantum uctuations destroy the correlation of spin orientations at distances noticeably larger than this radius. As the critical point Tc is approached from above, the correlation radius grows, accompanied by the stronger and stronger cooperative effects that eventually result in the formation of a new ordered phase at T = Tc , and the material is ferromagnetic below Tc . CORRELATION TIME

Time interval τ during the course of which the value of the second-order correlation function decreases by the factor of e = 2.718. The stationary random quantity u(t1 ) (e.g., thermal displacement of the crystal atom) correlates with its value u(t2 ) at a later time t2 if the ensemble average value of the product c(t1 , t2 ) = u(t1 )u(t2 ) = 0. The quantity c(t1 , t2 ) is called the second-order correlation function. For stationary processes, e.g., lattice vibrations, c(t1 , t2 ) depends only on the time difference τ = t1 − t2 , and the dependence c(τ ) is such that |c(τ )| |c(0)|. For some classes of random quantities c(τ ) has an exponential dependence on τ : c(τ ) = c(0) exp(−τ/τc ), where

218

CORROSION

τ c is the correlation time, or the time constant associated with the relaxation decay of correlations. The quantity c(τ ) does not always have an exponential dependence on τ . For example, the single-phonon correlation function ui (t1 )uj (t2 ) is not exponential in the low-temperature region where the anharmonicity of vibrations is negligible (see Anharmonic vibrations), and its correlation time corresponds to the reciprocal width at half-maximum of the Fourier transform c(ω) = ∞ c(τ ) exp(iωτ ) dτ . −∞ CORROSION (fr. Lat. corrodo, gnaw away) Physicochemical interaction of a solid and a

medium (liquid, gas) resulting in the degradation of the material operating properties. During corrosion the oxidation of source material or its individual components (anode process) occurs with a simultaneous cathode process, i.e. the reduction of medium components by the uptake of electrons released at the anode reaction. Corrosion takes place irregularly on the surface due to the chemical and structural inhomogeneity of an actual solid body, and it is accompanied by product formation (including compact non-conducting depositions) from the elements present in the solid composition and surrounding medium. The local corrosion rate is limited by the rate of the slowest process, in accordance with the mixed electron potential on the surface (corrosion potential) which is being generated for conditions during which the rates of anode and cathode processes are equal. On the basis of the type of external exposure on the solid, which accelerates the breakdown process, we can distinguish electrochemical corrosion (during electric current ﬂow), stress corrosion, and photocorrosion (during illumination). In the latter case, for oxidation–reduction processes charge carriers are excited in the solid, and corrosion products participate in generating a new phase on its surface. There are external and internal photoeffects, such as the photoactivation of anode dissolution of n-type silicon, at a rate which is limited by the generation of holes at the Si surface layer. The nature of the surrounding medium determines different corrosion types: electrochemical, gas, atmospheric, soil, biological, sea, and so on. During high-temperature gas corrosion solid oxidation products (scale) are usually formed. In such

conditions the oxidizing agent diffuses through the scale to the solid surface, and solid components diffuse in the reverse direction. If the transport of components through the scale is impeded its primary layers show a protective, anticorrosion effect at the subsequent contact with the medium. The corrosion rate can be varied by introducing into the corrosion active medium some chemical compounds, e.g., inhibitors which decrease the rate of corrosion, or promoters which increase it. The protective mechanism of inhibitor molecules usually consists in their ability to diminish the limiting step rate of the corrosion process at adsorption on a solid surface, or to promote the formation of a protective coating which prevents corrosion (see corrosion protection). Volatile inhibitors which protect engineering industry products from atmospheric corrosion have gained wide-spread acceptance: corrosion inhibitors are added to lubricants, oils, fuel, brake ﬂuids, and emulsions that considerably decrease material losses from corrosion processes. The formation of anticorrosive coatings can also be promoted by alloying materials (steels) with special additives (Cr, Al, Si). CORROSION, CONTACT See Contact corrosion. CORROSION CRACKING Brittle failure of a metal in a corrosive medium

with a static ﬁeld of tensile stresses present in the lattice. The onset of corrosion cracking requires the presence in the medium of a component which creates the conditions for sharp localization of the corrosion process on the metal surface, and at structural defects. Corrosion cracking takes place in solutions of electrolytes (sulﬁde, chloride cracking, caustic embrittlement of steel, hydrogen cracking of steel in acid, etc.); in gases (hydrogen, ammonia), and in molten metals (mercury). A measure of a metal stability against corrosion cracking is its limiting tension loading with a particular base test, or more precisely, the critical coefﬁcient of stress intensity (cracking stability) KSI in the corrosion crack vertex below which the crack does not grow. The rate of crack growth is determined by the anode (active) metal dissolving rate in the crack vertex, the possible decrease of adsorption strength, hydrogen saturation of the

CORROSION OF METALS

metal volume before the crack, and the value of the stress intensity. The relative role of the corrosion factors differs for different metal–solution systems. In a hydrogen atmosphere at high temperature with cathode hydrogen saturation the main role is played by the hydrogen saturation of the metal, i.e. hydrogen brittleness. CORROSION FATIGUE

The degradation of a metallic crystal lattice in a corrosive medium at exposure to a variable ﬁeld of tension stresses. Corrosion fatigue is a measure of the limit of permissible cyclic metal loads in a given corrosive medium based on the number of selected load cycles, or on the critical intensity coefﬁcient of cyclic tension stresses below which the growth of cracks is not observed. The corrosion fatigue limit is much lower than that of metal fatigue in an inert medium. An increase of metal strength through a long-term base test, as a rule, does not cause an increase in corrosion fatigue in a given metal–medium system. Depending on the frequency and loading level, we can distinguish low-cycle and high-cycle corrosion fatigue. The types of loading are the stretching from zero, expansion–contraction, arching (pure and cantilever), torsion with different forms of loading cycles (sinusoidal, rectangular, trapezoidal, symmetric, asymmetric). Taking into account the presence of residual technology loading in real systems, the most general is asymmetric loading, which is also the most dangerous for a metal–medium system that is susceptible to corrosion cracking. Methods for limiting the increase in corrosion fatigue are the creation of compression stresses in the surface layers of a construction, surface alloying or use of protecting coatings, change of corrosion medium composition, lowering of the temperature, application of inhibitors, and electrochemical protection. CORROSION, INTERCRYSTALLINE See Intercrystalline corrosion. CORROSION OF METALS Metal destruction due to chemical or chemico-

physical interaction with a corrosive medium. A common cause of the corrosion of a metal (M)

219

is a chemical oxidizing reaction, e.g., by dry oxidizing gases in accordance with the following reaction: nM + mO2 = Mn O2m .

(1)

During the corrosion of metals in electrolytic media (electrolytic solutions, including those impregnated by porous bodies (e.g., soils), electrolytic melts) Mz+ cations transfer into the medium to form compounds with different solubilities. There are corresponding characteristic reactions in acidic and neutral aqueous solutions: M + zH3 O+ = Mz+ + 0.5zH2 + zH2 O,

(2)

M + 0.25zO2 + 0.5zH2 O = Mz+ + zOH− . (3) A metal–medium system, as a rule, is thermodynamically unstable, and hence it is an environment for the spread of corrosion. Despite successes in the development of materials with increased corrosion resistance, anticorrosive coatings, and other corrosion protection methods, the problem of metal corrosion persists because of the deﬁciencies of materials, the greater severity of the conditions imposed on metal usages, and other reasons. Economic losses from the corrosion of metals result from the decreased machinery and communications productivity, direct metal losses, and so on. In the case of the formation of thin ( Tc .

The formation of a Cottrell medium causes dislocations to become pinned. To separate dislocations from the impurity medium the stress σc ≈ W0 /b3 is needed, and σ0 ≈ 1 GPa for typical values W0 ≈ 0.1 eV. COULOMB EXPLOSION in a solid Expulsion of positive ions driven by Coulomb

Equipotential lines W (r, θ ) = const for an edge dislocation. Each circle is for a particular W0 value. The array of lines for c(r, θ ) = const is similar.

repulsion when several nearby atoms are simultaneously ionized. The Coulomb explosion may be caused by the simultaneous ionization of two atoms. The formation of an electron vacancy in an internal electron shell of an atom affected by ionizing radiation, or the appearance of a slow multicharge ion inside the solid or at its surface, can result in cascades of Auger transitions (see Auger effect). These may be both “vertical” in a single atom, and “horizontal” (when the growing positive charge is distributed among neighboring atoms, and ultimately results in a Coulomb explosion as well). A Coulomb explosion in a solid produces point defects, defect clusters can also form, and the surface of the solid may suffer sputtering. Coulomb explosions contribute to the degradation along the trajectories of heavy accelerated ions or fragments of nuclear ﬁssion. The Coulomb explosion in metals is not effective because of the rapid “dispersal” of microscopic positive charge in a metallic conductor. The rates at which charges

222

COULOMB GAP

are neutralized in insulators and semiconductors with their low concentration of current carriers are much slower, and the inﬂuence of the Coulomb explosion on the formation of defects may be much more effective. COULOMB GAP A gap in the density of states g(E) of electron excitations around the Fermi level μ in a disor-

dered system with localized electrons, e.g., the gap in weakly doped compensated or amorphous semiconductors that results from the long range Coulomb interaction. An important characteristic of the Coulomb gap is its energy Δ. Provided that the Coulomb interaction energy between two localized current carriers separated from each other by an average distance (averaged over all localized carriers) remains small in comparison with the characteristic spread of the energy levels, the 1/2 value of Δ is of the order of e3 g0 /ε3/2 in a three-dimensional system. Here ε is the dielectric constant, and g0 is the density of states at the Fermi level in the absence of the electron–electron Coulomb interaction (see Fig.). Such a situation is found in a crystalline semiconductor for both strong and weak compensation, and also in amorphous semiconductors. In the case of medium compensation in a weakly doped semiconductor Δ is comparable to the overall width of the impurity band, and the Coulomb gap is more strongly expressed. The density of states at the Fermi level vanishes only for zero temperature. With increasing temperature the Coulomb gap “closes” and totally vanishes as soon as the thermal energy kB T reaches several tenths of the value of Δ. This gap manifests itself in experiments that measure the

Density of states g(E) of an amorphous semiconductor near the Fermi level μ.

hopping conductivity versus hopping distance in

regimes where that the principal contribution to the electrical conductivity arises from states in the energy band that are within the energy range Δ from the Fermi level. A technique to observe the Coulomb gap directly is tunneling spectroscopy. COULOMB PSEUDOPOTENTIAL See Morel–Anderson Coulomb pseudopotential. COVALENT BOND, homopolar bond

A particular type of chemical bond formed between similar atoms or atoms whose properties differ very little from each other, when the pairing (overlap) of the electron shells of neighboring atoms takes place without any appreciable exchange of the electric charges of the two atoms. A typical example of a covalent bond is the bond in a hydrogen molecule. The two-electron wave function of such a molecule can be written down in the simplest Heitler–London approximation as follows: ψ(r1 τ1 , r2 τ2 ) = ψa (r1 )ψb (r2 ) + ψa (r2 )ψb (r1 ) × χa (τ1 τ2 ),

(1)

where ψa and ψb are the 1s-type one-electron wave functions centered on the a and b atoms, respectively, and χa is the antisymmetric wave function of the spins. The difference between the eigenenergy obtained from solving the Hamiltonian of the molecule constructed using the wave functions (1) and twice the electron energy in an isolated atom corresponds to the covalent bond energy. A similar construction is used for the wave function of two electrons of a σ -bond between nearest neighbor atoms in homopolar crystals (diamond, gray tin, germanium, silicon) as well as in the AIII BV and AII BVI compounds (ψa and ψb are distinguishable in this case, appearing as sp3 hybrid functions of the valence electrons of the atoms involved). If the crystal is formed from atoms belonging to different groups of the periodic system then there can be a greater or lesser admixture of ionic bond character in the bond, and this will be termed an ionic-covalent bond.

CRACK

COVALENT CRYSTALS Crystals held together by covalent interatomic

chemical bonds. Covalent crystals are most often formed by elements of Group IV and adjacent groups of the periodic system, and are characterized by a tetrahedral (sp3 ) hybridization of orbitals, with the chemical bonds formed by singlet pairs of electrons localized in the space between nearest neighbor atoms (see Covalent bond). Because these bonds display distinct direction and strength, covalent crystals posses a high hardness and elasticity, some of them being brittle. Covalent crystals usually exhibit a high thermal conductivity. The most typical covalent crystal is diamond (C); others are silicon (Si), germanium (Ge), gray tin (α-Sn), and a range of compounds formed from elements alongside group IV of the periodic system. These are: the AIII BV compounds, e.g., borazon (BN), GaAs, GaSb, InAs and AlP; AII BVI compounds, such as beryllium oxide (BeO), zinkite (ZnO), sphalerite (ZnS), CdTe, etc. All these compounds are semiconductors, with their energy band gap varying between 0.2 to 2–4 eV. As the elements move apart horizontally in the periodic system, like in the AI BVII compounds: CuCl, CuBr and AgI, the covalent nature of the bond weakens and it becomes partially ionic in character. Moving vertically down the periodic table some metallic features appear: for instance, crystals of white tin (β-Sn) are virtually metallic. Covalent crystals of triple and more complex compounds which likewise possess tetrahedral atomic coordination also exhibit some degree of metallic behavior; examples are chalcopyrite (CuFeS2 ), stannite (Cu2 FeSnS4 ), CdSnAs2 , etc. Covalent crystals with octahedral coordination are exempliﬁed by PbS, PbSe, SnTe, Bi2 Fe3 , Bi2 TeS2 , etc. Many crystals are heterodesmic (see Heterodesmic structures), i.e. the atoms in their crystalline structure have bonds of different types. Thus, graphite crystals are covalently bonded within the hexagonal layers, while the bonds between the layers are of the van der Waals type. The structure of elements close to Group IV, such as P, S, Se or Te, may be described in a similar way: the atoms form covalently bonded groups, but the groups themselves are bonded together by van der Waals forces. Many covalent crystals are widely used in technology: native and synthetic

223

diamonds as abrasives and silicon crystals of the highest purity serve as the basis of semiconductor electronics together with the covalent crystals Ge, GaAs, InSb, etc. COVALENT CRYSTALS, PLASTIC DEFORMATION See Plastic deformation of covalent crystals. COVALENT RADIUS

A parameter of the size of an atom in covalent compounds (see Covalent crystals). The covalent radius is deﬁned as half the distance between two identical atoms held together by a covalent chemical bond. The length of a single chemical bond between differing atoms can be evaluated as a sum of the covalent radii of the corresponding atoms. A commonly employed system is the set of Pauling covalent radii which are deﬁned for atoms in tetrahedral crystals such as diamond (C) and sphalerite (ZnS) (see Atomic radius). COVARIANCE

The quality of physical quantities found in reference frames of a certain theory being transformed to other frames according to representations of the invariance group of this theory. For instance, in special relativity Lorentz covariance presumes using physical quantities that transform as relativistic vectors (e.g., 4-vectors), tensors, spinors, etc. via Lorentz transformations. Gauge covariance is referred to in the case of a gauge transformation (see Gauge invariance). Covariance also implies the conservation of the form of an equation with respect to the transformations of the invariance group. For instance, the covariance of the form of the equations of general relativity implies that the equation appears the same in any four-dimensional reference frame, even though the speciﬁc equation coefﬁcients can (covariantly) change with a space–time transformation. CRACK

A disturbance of continuity of a solid which is localized along a certain surface; a plane defect with broken molecular bonds along its edges. There is a singularity at the crack tip which under mechanical loading leads to stress concentration

224

CRACKING

√ proportional to 1/ r where r is the distance from the crack tip. Depending on the shape of the displacement between the edges, cracks are classiﬁed as rupture cracks, and longitudinal and transverse shear cracks. In respect to stability, cracks are divided into equilibrium (i.e. subcritical which do not grow spontaneously) and nonequilibrium (i.e. overcritical which can propagate under action of the elastic potential accumulated by the system). In respect to the involvement of plastic deformation, cracks are divided into brittle (i.e. not connected with material yield) and tough (see Brittle failure, Tough failure) with a certain portion of plasticity. There are microscopic and macroscopic cracks. Classed among the former are sizes of cracks from the atomic scale to the subgrain scale. Referred to the latter are cracks whose dimensions are greater, by at least an order of magnitude, compared to the structural elements of the solid such as subgrains, crystallites, etc. The ﬁrst stage of failure is microcrack nucleation. There are two kinds of microcracks differing in the shape: elastic (force) cracks and dislocation cracks. The former are like an incision along an atomic plane with broken molecular bonds from one tip to another, and the surfaces are opened by the applied stresses. A particular feature of such a crack is its instability. It can spontaneously collapse after the stress release, so that it cannot exist in an unloaded body. A dislocation microcrack is an empty nucleus of a superdislocation with a large Burgers vector. It is mechanically stable, and can occur in an unloaded body. The nucleation of this type of crack is determined by collective dislocation processes. There is a series of crack nucleation mechanisms: dislocation junction, braked shear, opening of bent slip band, interaction of dislocations at crossing slip planes and at broken walls of subgrains, generation according to the scheme of opposite clusters and interacting twin layers, and so on. The second stage of microcrack development (subcritical growth) is also fully determined and controlled by dislocation phenomena. Its essence is the “falling” of dislocations in the crack that induces the growth of its Burgers vector. There are several mechanisms for this process: the crack is initiated by the slip band approaching a tip; two slip bundles adjoin the crack; an accumulation

in the crack of dislocations from the slip bands stopped by boundaries. At this stage of failure a substantial role is played by rotation processes when individual grains and their groups are able to rotate freely about the crack tip (see Plastic twisting deformation). Subcritical growth of the macroscopic crack proceeds via the same mechanisms with the added feature that the plastic deformation involving a large volume leads to the appearance of a system of secondary microcracks and pores prior to the main crack formation. The failure proper is then effected through a merging of the crack system into a common one by the tough rupture of bridges. The third stage of crack development, involving overcritical growth, proceeds with completely or almost completely suppressed plasticity at the vertex. Here, the spreading of the crack exhibits a distinctly elastic and overstructural character, with the limiting velocities of growth determined by the elastic constants of the medium, and by the sample geometry. The maximum possible velocities of failure, according to different evaluations, vary from 0.53 of the transverse elastic wave velocity to 0.38 of the longitudinal wave velocity. The limiting velocity of the crack, equal to the velocity of surface Rayleigh waves (see Surface acoustic waves) is considered to be the preferable index. In the case when additional feeding of the crack vertex by elastic energy is not mediated by the elastic waves that spread through the destructible material, but is performed directly, e.g., by plasma expansion at the vertex of crack under the effect of a laser beam, the velocities of crack propagation may be considerably higher, and may even exceed the sound velocity. See also Brittle crack, Nucleating crack, Submicrocracks, Tough crack, Wedge-shaped crack. CRACKING

The process of extraction of products with lower molecular mass from hydrocarbons, mainly of petroleum origin. The ﬁrst and foremost high tonnage industrial application of the process is extraction of motor fuels. Many processes of cracking are run in the presence of solid catalysts (catalytic cracking). The catalysts most often used are highly porous synthetic aluminosilicates containing Al2 O3 and SiO2 in various proportions.

CREEP

Complex sets of reactions involved in catalytic cracking always include the formation of new solid phases which poison the catalysts. These are cokes, and their mass can reach several per cent of the catalyst mass. To remove cokes the silicaaluminas are oxidized with air, or an air–vapor mixture (process of catalyst regeneration). CRACKING CORROSION See Corrosion cracking. CRACK RESISTANCE The same as Fracture toughness. CRAIG EFFECT (D. Craig, 1955)

Changes in the spectra of electronic and vibrational excitations of a molecule located in a crystal matrix. The inﬂuence of the local crystal e ld and intermolecular interactions results in a partial splitting of degenerate states, and changes of selection rules, thereby producing a larger number of observable bands in the optical spectra, and also changes their relative intensities and polarization properties. These phenomena were initially encountered during applied studies of molecular crystals. CREEP

Property of a solid to increase strain or to deform during the course of time under the action of a constant external stress or load, usually at an elevated temperature. The relationship between strain and time is given by the creep curve, which is arbitrarily divided into characteristic regions. At the moment of applying stress an instantaneous strain is induced; then comes the stage of initial creep or transient creep. The rate of deformation decays at this stage. At the second stage (secondary creep) the rate of deformation is constant. The third stage is characterized by an increase of the creep rate, then the process ends with failure. The shape of a creep curve depends on the temperature, stress, initial structure, and stability of the initial structure. Depending on these factors, there are four kinds of creep with different deformation mechanisms. (1) The ﬁrst kind of creep is observed if the applied stress is lower than the critical shear stress. This type of creep is called elastic creep or reversible creep. It is adequately described by the

225

equation ε = εl + ε0 [1 − exp(−t/τ )], where εl is a purely elastic strain (see Elasticity), t is the time after loading, ε0 and τ are constants. The second term of this equation stands for inelastic strain, which tends to ε0 . After load release the strain completely regains its value due to inelastic creep. One of the mechanisms, which provides an explanation for inelastic creep, proposes the diffusive transfer of impurity interstitial atoms into crystal lattice interstices, which are stretched under the action of the applied stress (see Diffusion). The strain ε0 is proportional to the applied stress, and to the concentration of impurity interstitial atoms. After release of stress interstitial atoms tend to become uniformly arranged at interstices, and the strain is restored. Inelastic creep may also be caused by short-distance transfer of dislocations, which does not involve abstraction from pinnings. (2) At stresses that are higher than the critical shear stress, the second kind of creep is observed in the low-temperature region, called logarithmic creep or low-temperature creep, and described by the equation: ε = α ln(1 + νt), where α 0 and ν 1 are constants. This relation is valid up to very slight strains (ε 0.2%). So far it is unknown whether logarithmic creep is followed by secondary creep, because tests to conﬁrm this are very time consuming to carry out. (3) As the temperature exceeds T G (for metals T G ≈ 0.5T melting and decreases with increased load) the third kind of creep is observed: high-temperature creep. The mechanism of hightemperature creep is related to the creeping of dislocations, and is controlled by processes that are determined by the rate of self-diffusion (motion of thresholds at screw dislocations, rate of creeping of dislocations around obstacles, etc.). High-temperature creep is described by the relation: ε = ε0 + βt m + Kt , where ε0 is the instantaneous strain, β and m are time-independent constants, 1/4 < m < 2/3 (according to Andrade (1910) m = 1/3), K and Kt are, respectively, the rate and strain at the ﬁrst stage. At this stage hardening dominates over dehardening, the density of dislocations increases, and the size of subgrains decreases; during the steady state the size of subgrains remains constant, whereas disorientation of subgrains increases in proportion to the increase of strain.

226

CREEP RESISTANCE

At the second stage of creep the duration and rate of deformation depend on the stress and temperature. The equation K = A exp[H /(k B T )] × sinh(Bσ )n , where T is temperature, σ is stress, A, B, n are constants, describes the temperature dependence and stress dependence of K. The activation energy H monotonically increases with the increase in temperature; for T > T G it is a constant equal to the self-diffusion activation energy. This means that at low temperatures diffusionrelated mechanisms of plastic deformation are activated. It has been found that slippage along the grain boundaries contributes signiﬁcantly to the creep at the second stage. The dependence of ε˙ is ∝ d 2 at low temperatures and ∝ 1/d at high temperatures, while at intermediate temperatures it takes the form k/d + Kd 2 , where k and K are constants, and d is the grain size. The inﬂuence of grain boundaries at elevated temperatures may be explained by localization of plastic deformation in border zones. The third stage of creep is prepared by structural changes, which take place at preceding stages. It is thought that acceleration of creep occurs because of an increase of stress that is related to the generation of a neck, the decrease of the actual cross-sectional area caused by accumulation of microcracks (see Cracks) and pores, or processes of recovery and recrystallization. (4) The fourth kind of creep, which is called diffusive creep, is observed at low temperatures and low stresses, and does not involve the transfer of dislocations, but is a result of directional diffusive mass transport. The rate of such creep, due to the self-diffusion or ﬂux of vacancies between external surfaces of the sample, has been calculated in works of F.R.N. Nabarro, C. Herring (1950) and R.L. Coble (1963). Taking into account the increase of creep rate caused by grain boundary diffusion, we obtain the equation: πδDg 5D σ Ω 1+ , ε˙ ≈ 2 Dd d kBT where D and Dg are the coefﬁcients of bulk and grain boundary self-diffusion, respectively, δ is the effective thickness of a grain boundary, and Ω is the atomic volume. Creep resistance of materials is characterized by the creep limit, i.e. the stress at which a certain

strain is achieved in a given time. Creep resistance depends on the type of interatomic bond, type of crystal lattice, stacking fault energy, grain structure, and other characteristics of the material. High creep resistance is the main factor determining the high-temperature strength of materials. See also Athermic creep, Diffusion mechanism of crystal creep, Radiation-induced creep. CREEP RESISTANCE See Creep. CRITERION OF LOCALIZATION See Anderson localization. CRITICAL CURRENTS in superconductors

The minimum value of the current Ic or current density jc at which the superconducting state is destroyed. Several types of critical currents are identiﬁed. In type I superconductors the value of Ic depends on the shape (geometry) of the sample. In particular, for a long enough cylindrical superconductor it is obtained from the condition that the azimuthal component of the magnetic ﬁeld of the longitudinal current, Bf = I /(2πa), reaches the value of the thermodynamic critical magnetic eld Bc (T ) at the surface of a sample of radius a. When I > Ic = 2πaBc (T ) the superconductor transforms to the intermediate state with a ﬁnite resistance. In type II superconductors the critical current density is determined by the pinning strength of the Abrikosov vortices, or by the ﬂuidity limit of the vortex lattice (see Vortex pinning). There is also a decoupling critical current at which the Cooper pairs are broken and the supercurrent ﬂow is terminated. The current velocity v = j/(eN0 ) (here j is the current density, N0 is the concentration of electrons in the metal) exceeds the critical velocity vc = Δ/pF , where Δ is the superconductor energy gap, and pF is the Fermi momentum (see Kinetic decoupling of Cooper pairs). Such currents may be reached in very thin superconducting ﬁlms and ﬁlaments, the magnetic ﬁeld of the current at their surface being lower than Bc (T ) in type I superconductors, or such that their thickness is smaller than the London penetration depth of the magnetic eld of a type II superconductor. However, recalling the presence of inhomogeneities, it becomes clear that

CRITICAL EXPONENTS

the destruction of the superconducting state, and the recovery of the resistive state in thin ﬁlms and ﬁlaments are usually controlled by vortex pinning at these inhomogeneities. Finding ways to increase critical currents is one of the most important tasks of applied superconductivity. CRITICAL DISORIENTATION OF DISLOCATION SUBBOUNDARY

The threshold value of the disorientation angle in a cellular structure at which, similar to grain boundaries, cell boundaries start to resist the movement of dislocations. The concept of critical disorientation of dislocation subboundaries resulted from comparing the mechanical properties of metals during the formation of the sublattice dislocation structure (either cellular or fragmented) that develops in the process of plastic deformation (see Fragmentation). While the overall density of dislocations remains unchanged with growing plastic deformation, they undergo redistribution in the process. The number of dislocations in the body of the subgrain diminishes, their density at subboundaries increases and the angle of disorientation of the adjacent cells grows, so that dislocation slip to large distances becomes more difﬁcult. The critical value of the angle of disorientation, θcr , usually remains within several degrees, and may be estimated from the expression Ky 2 (1 − ν)2 2πn θcr = , G 0.45b where G is the shear modulus, ν is the Poisson ratio, Ky is a constant value from the Hall–Petch equation (see Petch relation), b is the Burgers vector, n is the ratio of the effective slip length L to cell size l. Following the growing plastic deformation the number of subboundaries in the already formed dislocation cells increases, such that their disorientation angle is either equal to or already exceeds the value of θcr . This results in a signiﬁcant strengthening of the material, while the temperature of cold brittleness simultaneously decreases, which means that the formation of a disordered cellular dislocaton structure signiﬁcantly improves the overall mechanical properties of the material. For such a structure to form certain conditions have to be met, and the strain should take place within the temperature range of warm deformations.

227

CRITICAL EMBRYO, critical bubble

Seed or embryo of a stable thermodynamic phase in unstable equilibrium with its surrounding metastable phase (see Metastable state). The

radius of a spherical critical embryo is given by rE =

2γ v 2γ Tc (vM − v) = . μM (P ) − μ(P ) q(T − Tc )

Here γ is the coefﬁcient of surface tension; v, v M are the atomic volumes; μ and μM are the chemical potentials (see Thermodynamic potentials) for the embryo and the metastable phase, respectively; P is the external pressure, Tc is the phase equilibrium temperature; q is the latent heat of the phase transition from the metastable phase to the embryo phase. Only embryos above the critical size continue to grow. The process of growth, stable with respect to ﬂuctuations, sets in at r > r E + [k B T /(4πγ )]1/2 . For a supercritical embryo (r > r E ) to form it has to penetrate the thermodynamic potential barrier 4πrE2 γ /3. See also Nucleation at phase transitions, Crystallization. CRITICAL EXPONENTS, critical indices

Power law indices or exponents deﬁning the dependency of dynamic and thermodynamic parameters such as the external ﬁeld h, etc., on the reduced temperature, τ = T /Tc − 1, etc. around a second-order phase transition point (Tc ). Critical exponents only characterize the principal, leading asymptotes of these quantities. When τ, h change the system may pass through several regimes or phases, each of them described by its speciﬁc set of critical exponents. For example, when approaching the triple critical point the system passes through a transition region in which its behavior changes from that typical of a second-order phase transitions to a tricritical (around that point) behaviour. Critical exponents used to describe thermodynamic (statistical) properties of the system deﬁne the temperature dependences of the speci c heat cp ∝ |τ |−α , the order parameter M ∝ (−τ )β , the susceptibility χ ∝ |τ |−γ , and the correlation length rc ∝ |r|−ν , where the exponents β, γ , ν > 0. The critical exponents of anomalous dimensions for ﬂuctuations of the order parameter characterize the law by which the correlation func-

228

CRITICAL FLUCTUATIONS

tion decreases with distance r for r rc , G(r) ∝ r −(d−2+η) , where d is the dimensionality. For T = Tc the critical exponents describe the behavior of the system in the external ﬁeld h: cp ∝ h−ε , M ∝ h1/δ , rc ∝ h−μ (δ, μ > 0). Critical exponents are related to each other via certain algebraic expressions called scaling relations: α + 2β + γ = 2, βδ = β + γ , ε(β + γ ) = α, μ(β + γ ) = ν, ν(2 − η) = γ , γ d = 2 − α (see Scaling invariance hypothesis). Critical exponents also describe the kinetic (dynamic) properties of the system around Tc . For example, the relaxation time t (k, T ) of ﬂuctuations of the order parameter with wave vector k has the form t (0, T ) ∝ |τ |−y and t (k, Tc ) ∝ k −z in the critical region. Scaling relates these exponents to each other: y = zν. Critical exponents are universal values, i.e. they do not depend on the nature of the particular phase transition, or on the speciﬁcs of the physical system. They depend, instead, only on the number of components of the order parameter, and on the dimensionality d of the space. Critical uctuations become insigniﬁcant for d > dc , where dc is the so-called upper critical dimension, so that the critical exponents coincide with those provided by the Landau theory of second-order phase transitions. At d = dc ﬂuctuations generate multiplicative logarithmic corrections to the results from the Landau theory. If d < dc the corresponding critical exponents differ from those prescribed by the phenomenological theory of phase transitions. Their values may be (approximately) calculated using the techniques of high temperature expansions within the renormalization group method, in particular through expansions in powers of ε = dc − d (epsilon expansion), in terms of the spherical model, employing the 1/n expansion approach, and by other techniques. CRITICAL FLUCTUATIONS

Particularly strong thermodynamic ﬂuctuations of the order parameter and other physical variables observed near second-order phase transitions. The correlation length of these ﬂuctuations and their respective relaxation times grow without limit when approaching the transition point, thus reﬂecting destabilization of the corresponding phase, and the stronger role of the cooperative effects in forming the dynamics and thermodynamics of

the crystal. Much effort has been expended toward explaining the strong nonlinear interactions of critical ﬂuctuations (see Renormalization group method, Epsilon expansion). Experimental studies of critical ﬂuctuations by neutron diffraction, optical, radiospectroscopic, and other techniques yield rich data on the behavior of materials in the critical region. CRITICAL MAGNETIC FIELDS in superconductors

Values of applied magnetic ﬁeld strength (that depend on superconductor shape) above which the character of the penetration of the magnetic ﬁeld into the superconducting material changes, or the sample reverts to the normal (nonsuperconducting) state. One distinguishes between the thermodynamic critical magnetic eld Bc in type I superconductors (see Meissner effect), and the lower critical eld, Bc1 , the upper critical eld, Bc2 , and the third critical eld Bc3 in type II superconductors. See also Mixed states. CRITICAL PHENOMENA

Speciﬁc effects observed in the neighborhood of second-order phase transition points. One distinguishes between static and dynamic critical phenomena. Among the ﬁrst are the anomalies of the thermodynamics of crystals, and features in the behavior of static kinetic coef cients. Examples of static critical phenomena are: sharp increase in the magnetic permeability of ferromagnets as the phase transition point Tc is approached; anomalous temperature dependence of the speci c heat, elastic moduli, etc.; increase in the electrical conductivity of normal metals near superconducting phase transitions; and temperature anomalies in the speciﬁc heat of ferroelectrics. Dynamic critical phenomena involve the dynamic susceptibility, a sharp increase in relaxation times as Tc is approached (critical slowing down), anomalies in Raman scattering of light, in inelastic neutron scattering, in X-ray scattering, and in Mössbauer spectra (see Mössbauer effect). Sometimes critical phenomena are understood in a narrower sense, as effects produced speciﬁcally by critical uctuations of the order parameter. The susceptibility χ , the order parameter M, and the speciﬁc heat C, all behave as power law functions of the reduced temperature τ = (T − Tc )/Tc

CRITICAL STATE

around the critical point Tc : χ ∝ |τ |−γ , M ∝ |t|β , c ∝ |t|−α . Second-order phenomenological theory of phase transitions predicts the values α = 0, β = 1/2, γ = 1 for these power law indices called critical exponents, but it does not take ﬂuctuations into account. Experiments usually yield the ranges −0.1 < α < 0.1, 0.3 < β < 0.4, and 1.2 < γ < 1.4 for three-dimensional (non-layered, non-quasi-one-dimensional) systems. Speciﬁc values of the critical indices depend on the number of components of the order parameter. CRITICAL POINT

A point associated with a second-order phase transition. When the transition occurs during a temperature change the critical point corresponds to a critical temperature. Examples are the Curie point of a ferromagnet, and the Néel point of an antiferromagnet. The critical point can also be the value of an electric or magnetic ﬁeld which induces a change in phase, such as the upper and lower critical magnetic ﬁelds of type II superconductors. CRITICAL POINT, TRIPLE See Triple critical point. CRITICAL PORE SIZE Size of a pore in unstable equilibrium with

its surrounding environment. Smaller pores shrink and heal (see Healing of defects), while larger sizes grow. The critical radius of a spherical pore r cr depends on the coefﬁcient of surface tension γ , the density of point defects, their mobility, the nature of their elastic interaction with the pore (see Elastic interaction of defects), the gas pressure inside the pore and outside the sample, and other factors. For example, we have r cr = 2γ /[P + k B T N0 ln(1 + c/c0 )] in the presence of extra vacancies (vacancy concentration c, equilibrium concentration c0 ). Here P is the difference between the pressures inside the pore and outside the sample, k B is the Boltzmann constant, N0 is the number of atoms per unit volume of material. In polarized substances (with electric or magnetic moments) the pore tends to stretch along the moment direction. The equilibrium ratio of pore axes is determined by competition between the growing surface energy and

229

the diminishing ﬁeld energy as the lines of force ﬂatten, so that ratio grows for larger pore volumes. As the pore enlarges it sucks in more and more energy from the ﬁeld, and it eventually reaches the critical size V = V cr , where 1/3 Vcr = 0.476γ (ln(0.309/N 7/6 ))1/6 /(M 2 N 7/6 ). The principal axes of the demagnetization factor tensors of the sample and pore (see Demagnetization) are assumed to coincide. Here M is the moment per unit volume, and N is the principal value of the sample demagnetization tensor along the pore axis. As a rule, the segregation of impurities in the pore surface layer lowers the surface tension and results in a lower r cr . CRITICAL REGION, critical temperature range

A ﬂuctuational range in the neighborhood of a phase transition, located in the phase diagram adjacent to the second-order phase transition line, or to the critical point, where the thermodynamics and dynamics of the system are strongly affected by critical uctuations of the order parameter. The size of the critical region is characterized by the Ginzburg number, and depends on the type of interatomic (electron, spin) interaction potential associated with the phase. The behavior of the system in the critical region may differ both quantitatively and qualitatively from that predicted by the Landau theory of second-order phase transitions. CRITICAL STATE

The limiting equilibrium state of a two-phase system at which the physical differences between the two phases vanish. For example, the α- and γ -phases of cerium with the same face-centered cubic lattice become identical in the critical state. The “liquid–vapor” case is quite well known. The critical state on a phase diagram corresponds to a critical point or critical line. When approaching that point critical uctuations of the density of the substance become very much larger, while the latent heat of a rst-order phase transition approaches zero. At the critical point itself the phase transformation occurs simultaneously throughout the entire system, similar to a second-order phase transition. The values of the state parameters for the critical state are called critical parameters, e.g., critical temperature, critical pressure, critical volume.

230

CRITICAL STRAIN

CRITICAL STRAIN, critical degree of deformation The extent of strain that results in a qualitative

change in the behavior of a material under a given external action (e.g., deformation which produces sample failure), or an irreversible change of the sample shape (i.e. plastic deformation). Sometimes one may speak about a critical deformation with respect to certain physico-chemical characteristics of a solid, in particular about a critical plastic deformation resulting in recrystallization, etc. CRITICAL SUPERCOOLING FIELD The value of the magnetic eld Bs at which

a sample in a normal (i.e. nonsuperconducting) metastable state transforms into a superconducting state. A type I superconductor can be supercooled, meaning that it can remain in the normal state when the temperature is below the superconducting transition temperature T c , and the applied magnetic ﬁeld is also below the thermodynamic critical magnetic eld B c . A further lowering of the applied ﬁeld to the value B s brings about a phase transition to the superconducting state. The effect is only observed in pure (type I) superconductors, and its magnitude is characterized by the ratio α = Bs /Bc < 1. In some superconductors (Al, In, Sn, etc.) the extent of the overcooling may be quite signiﬁcant, and indium has been supercooled down to α < 0.1. CRITICAL TEMPERATURE

A temperature corresponding to a critical point, i.e. a point on a phase diagram at which the equilibrium curve for two phases in contact comes to an end. The concepts of critical temperature and critical point were introduced by D.I. Mendeleev (1860). The critical point is an isolated point of a second-order phase transition, and more generally Tc is often understood as the temperature of second-order phase transitions, including cases when the phase diagram contains a line or even a range of continuous phase transitions. The thermodynamic potentials of the system, which are functions of thermodynamic variables (such as temperature, volume, electric or magnetic polarization), feature singularities at T = Tc . While approaching Tc their derivatives, such as susceptibility, speci c heat, etc., may grow without limit. In the neighborhood of Tc the temperature dependences of thermodynamic variables are described

by power law functions (see Critical phenomena, Scaling invariance hypothesis). Several examples of critical temperatures are: transformation of a metal to a superconducting phase, transitions to magnetically ordered or ferroelectric states (Curie point), and transformation of a liquid to a super-

ﬂuid state. CRITICAL TEMPERATURE OF SUPERCONDUCTORS

Transition temperature Tc from the normal state of ﬁnite resistance R to the superconducting state of zero resistance, which is speciﬁc for each superconductor (see Fig.). In the absence of a magnetic ﬁeld the transformation corresponds to a second-order phase transition. For the phonon mechanism of superconductivity the value of Tc depends on the magnitude of the electron–phonon interaction constant λ. This interaction involves the attraction between pairs of electrons in the vicinity of the Fermi surface with the formation of Cooper pairs, despite repulsion from the Coulomb interaction. The calculation of Tc from ﬁrst principles is so complex that Tc is usually estimated from its dependence on various parameters in terms of simpliﬁed models. The most useful approach involves the Bardeen–Cooper–Schrieffer theory (BCS) which yields the following expression for Tc : Tc ≈ ΘD e−1/g . Here Θ D is the Debye temperature, and g is a dimensionless positive coupling constant, with the BCS model value given by g = N(EF )(Vph − Vc ), where N(EF ) is the density of states of electrons at the Fermi level EF , Vph and Vc are the

Critical temperature of superconductors.

CROSS-RELAXATION

matrix elements of the electron–phonon interaction (second order in perturbation theory) and the Coulomb repulsion, respectively. Note that g > 0 for Vph > Vc , corresponding to the BCS criterion for superconductivity. A more accurate accounting for the Coulomb repulsion in the energy range near EF results in its signiﬁcant weakening (the logarithm ln[EF /(ωD )] becomes large (see Bogolyubov–Tolmachyov logarithm) and a softening of the superconductivity criterion Vph > Vc∗ ≡

Vc . 1 + N(EF )Vc ln[EF /(ωD )]

McMillan (1968) was the ﬁrst to make approximate calculations of Tc for the cases of intermediate and strong coupling in the limit λ 1. He used the integral Eliashberg equations and obtained: ΘD 1.04(1 + λ) , exp − Tc = 1.45 1 − μ∗ (1 + 0.62λ) where μ∗ = N(EF )Vc∗ is the Morel–Anderson Coulomb pseudopotential. CROSS-DEFORMATION INTERACTION, electron–phonon interaction in one-dimensional metals Interaction between conduction electrons and long-wave phonons in conductors exhibiting onedimensional electrical conductivity (one-dimen-

sional conductors). It is produced by modulation of a random static scattering ﬁeld of impurities or other defects by a sound wave. It is non-diagonal in the electron momenta at the Fermi surface of a one-dimensional metal, i.e. the sign of the electron velocity can change due to this interaction. It is similar to the common deformation interaction (A.I. Akhiezer, 1938) that is described by introducing an additional term Hd = λik uik into the Hamiltonian of an electron, where the strain potential tensor λik is of the order of the Fermi energy, eF , and uik is the strain tensor. The cross-deformation interaction results in the appearance of a new term in the Hamiltonian, its structure schematically represented by Hcd = Δik uik , where Δik is the complex crossdeformation potential tensor. In the case of the weak scattering of electrons at impurities (defects), the cross-deformation interaction appears

231

much weaker than deformation scattering, meaning | ik |/λik ∝ (eF τ )−1/2 for eF τ 1, where τ −1 is the frequency of electron–impurity scattering. However, since the deformation potential in one-dimensional metals does not depend on the quasi-momentum of the electron at the Fermi surface, and the electron energy bands do not overlap, the Coulomb interaction between the electrons almost completely screens the potential λik (to the accuracy of terms in (qa)2 of the order of magnitude (qa)2 1, where q is the wave number of sound, and a is the crystal lattice constant). Therefore, alongside the inertial interaction resulting from the Stewart–Tolman effect, the crossdeformation interaction is the principal type of interaction of electrons with long-wavelength sound waves in one-dimensional metals (see Electron– phonon interaction). CROSS-LINKING OF POLYMERS See Polymer cross-linking. CROSSOVER TRANSITIONS See Direct transitions. CROSS-RELAXATION Relaxation processes in spin and other quan-

tum systems with non-equidistant energy levels that control the reestablishment of equilibrium between these levels after excitation by a radiation source. For example, consider a spin system with two resonant frequencies ωa and ωb , so that the difference between them does not exceed their line widths. The process of cross-relaxation develops via mutual spin ﬂips, the so-called spin-ﬂip process, resulting from the magnetic dipole interaction between the spins. It can also involve spin exchange. The extra energy (ωb − ωa ) released during cross-relaxation is compensated by the increase of the dipole–dipole interaction energy of the spin system. Cross-relaxation processes may involve two qualitatively different types of spin systems: resonant frequencies ωa and ωb for different types of spins (Fig. (a)); and frequencies ωa and ωb for one and the same spin type (Fig. (b)). The latter case can occur in a system with S > 1/2 under the inﬂuence of a crystalline electric ﬁeld. The rate

232

CROSS-SECTION

Examples of cross-relaxation processes.

of cross-relaxation depends strongly on the difference between the energies of the respective levels, and becomes negligible when this difference exceeds the average dipole–dipole interaction energy. This phenomenon was initially observed during nuclear magnetic resonance in LiF where the rate of transfer of resonance saturation from the Li7 nuclei to the F19 nuclei depends on the value of the applied magnetic ﬁeld. The process of cross-relaxation can decrease the spin–lattice relaxation rate of a slowly relaxing system of spins by coupling them with another spin system that relaxes more rapidly via a much shorter spin–lattice relaxation time. Cross-relaxation is thus a mechanism for thermal contact between the two spin systems. For example, slowly relaxing nuclear spins can transfer their energy to the lattice much more rapidly if they undergo cross-relaxation with rapidly relaxing electronic spins. Beside these two-spin cases, cross-relaxation processes may involve larger numbers of spins, such as during dynamic nuclear polarization. CROSS-SECTION of a process, effective cross-section

A factor characterizing the averaged rate of change in the state of particles as a result of their interaction (scattering, dispersion, chemical, nuclear and other reactions). Let the velocity of one of two interacting particles relative to each other be v. Consider a system of N (cm−3 ) ﬁxed and n (cm−3 ) particles moving with relative velocity v in some initial state, with their ﬂux characterized by the intensity Φ = nv particles·cm−2 ·s−1 . The cross section σ of the process of transition from the initial to the ﬁnal state caused by particle interactions is determined from the relation dn/dt = σ ΦN = γ nN , where t is the time, and

γ = σ v is the probability of an elementary act of the process. The cross-section σ at a given Nnv deﬁnes the fraction of particles undergoing the change: dn/n = σ Nv dt . The change caused by scattering is usually characterized by a scattering angle θ , by the change of scattering energy of the particles, or by the value of their orbital angular momentum l after scattering. In the case of nuclear or chemical reactions, the system after the reaction is deﬁned by the ﬁnal reaction products and their states. If it is necessary to determine the rate of reaction product formation by characteristics from an inﬁnitesimal interval of values, then differential cross-sections are used. For example, scattering in the interval of angles [θ, θ + dθ], and scattering with power transmission from the incident particle to the scatterer in the energy (temperature) interval [T , T + dT ], are characterized by the differential cross-sections dσ/dθ , dσ/dT , etc. The corresponding total cross-sections are σ = (dσ/dθ) dθ and σ = (dσ/dT ) dT , where the latter integration is from T = 0 to T = Tmax , representing the maximal energy transferred in the interaction. The cross-section is deﬁned by quantummechanical probabilities of transitions between initial and ﬁnal states of the system under the inﬂuence of particle interactions, or by reasoning from the classical mechanics equations of motion. Both the scattering cross-section and cross-sections of various reactions often differ appreciably from the geometrical cross-sections of the interacting particles, or from dimensions deﬁned by the radius of action of a short-range force, and they can be much larger or much smaller than the geometrical dimensions. Thus, the elastic scattering of particles on a ball of radius r is characterized in classical mechanics by the cross-section σ = πr 2 corresponding to the maximal geometrical ball cross-section. Quantum theory takes into account the wave properties of scattering particles, and provides the expression σ = 4πr 2 for λ r (λ is the de Broglie wave length, λ = h/p, p is the scattered particle linear momentum). For λ r the cross-section is σ = 2πr 2 , and the contribution to the total cross-section of the order πr 2 gives the small angle scattering. For resonant scattering the elastic scattering cross-section reaches the value σl = 4πλ2 (2l + 1), and for slow particles with λ considerably exceeding the radius

CRYOCRYSTALS

233

of action of the force it is much greater than the geometrical dimensions of the system. This effect has a quantum origin. The opposite situation with the cross-section much smaller than geometrical dimensions is realized in reactions where there is an energy potential barrier between the interacting particles. Then, on the average, repeated approaches of reacting particles are necessary to overcome the barrier. A similar situation often occurs in quasi-chemical reactions involving point defects in a solid. CROSS SLIP

A transition of helical sections of dislocations from one slip plane with the normal n, to another one with normal m, if the line of the intersection of these planes is parallel to the Burgers vector of the dislocation b, i.e. [n × m]||b. A slip plane is the closest packed plane of a crystal on which dislocations glide. The cross slip appears, ﬁrst of all, near the obstacles for the usual dislocation slip. If such an obstacle is local, then after the motion within the cross slip plane the dislocation may return to the initial plane, i.e. the process of double cross slip takes place. It is experimentally established that in face-centered cubic single crystals the beginning of the third stage of hardening is associated to the fact that as a result of the stress concentration by single or multiple steps there appear areas of dislocation lines which may perform cross slip. The process of cross slip determines the creep of metals in the interval of moderate temperatures (e.g., for aluminum single crystals within the temperature range 0 to 100 ◦ C). CROWDION (fr. crowd)

A speciﬁc quasi-one-dimensional point defect of the type of an interstitial atom such that adjacent atoms are preferentially displaced along one of the directions of dense packing. The extra atom in a crowdion in a fully packed row displaces 5 to 10 atoms along the line by individual minimal distances (much shorter than the interatomic distance a, see Fig.). H. Paneth (1950) introduced the concept of a crowdion to describe self-diffusion in alkali metals with BCC lattices (with crowdion direction 111). Experimental data are available proving the existence of crowdions in FCC metals (Cu, Ni) at low temperatures (along the 110 direction). A crowdion may form during radiation.

Crowdion.

A dynamic crowdion appears when a pulse sufﬁcient to displace a neighboring atom is transmitted along a fully packed atomic row to one of the atoms of the crystal. A relay displacement then takes place, and the crowdion propagates along the direction of the transferred pulse. A site vacancy remains at the site of the initially dislodged atom. A dynamic crowdion is able to propagate a distance of the order of 103 a from the position of the initially dislodged atom. A static crowdion may remain stable in some crystals within a certain range of temperature. It propagates as a whole, and the process involves one-dimensional diffusion along the atomic line. Although a crowdion can travel a long distance, the displacement of an individual atom at each step in the displacement process is the same (equal to a). In its quantum-mechanical description the crowdion is a quasi-particle (a crowdion wave). CRYOCRYSTALS

Solidiﬁed gases, i.e. crystals formed by atoms or small molecules with weak intermolecular interaction forces, which therefore feature low crystallization temperatures. Their relative simplicity is convenient for studies of the general properties of the crystalline state of matter. Atomic cryocrystals – solid Ne, Ar, Kr, Xe are closest to theoretical models of crystals with central force interactions. They form face-centered

234

CRYOGENIC TECHNOLOGY

cubic lattices containing identical atoms interacting via valence forces of attraction, and dispersion forces of repulsion. Their low-frequency collective excitations are phonons, and their highfrequency ones are excitons. Solid N2 , O2 , CO, CO2 , CD4 , etc., are molecular cryocrystals. Their molecules may be considered nondeformable since their intramolecular forces are much stronger than the intermolecular ones. Due to their rigidity these molecules rotate as whole units. Non-central interaction forces (dispersion, exchange, and multipole) result in certain orientations of these molecules in the crystal lattice. Phase transitions mainly arise from changes in that orientational order. Their collective excitations are phonons (both acoustic and optical); librons (which appear only when some long range orientational order exists); bound intramolecular vibrations; excitons, and their combinations. If the central interaction dominates over the noncentral variety (e.g., in solid CD4 ), the breakdown of long-range orientation order (orientation melting) occurs within the solid phase. Regions of short-range orientational order may still persist in orientationally disordered crystals. With increasing temperature these regions shrink, and librons transform into weakly perturbed rotations. Of particular interest is solid oxygen, a molecular magnetic substance with particular structural features and collective excitations (magnons, biexcitons) that result from the uncompensated electron spin of its paramagnetic O2 molecule. Quantum crystals form a separate group of cryocrystals (3 He, 4 He, H2 , HD, D2 and CH4 ). The dynamics of the translational and rotational motions of these molecules deﬁes a classical description, being controlled by the laws of quantum mechanics instead. The weak intermolecular interactions, small size, and light mass of these molecules all combine to produce properties typical of cryocrystals: low crystallization temperature, strength and thermal conductivity, and high plasticity, compressibility, vapor pressure, and thermal expansion coefﬁcient. CRYOGENIC TECHNOLOGY

Branch of technology involving the development, manufacture and use of instruments and machines that produce and maintain low temperatures, and that can liquefy and separate various

gases. Industrial applications of cryogenic technology are numerous, since pure oxygen obtained by liquefying air and separating its gases at low temperature is widely used in metallurgy and other industries. Liquid nitrogen, also obtained from liquid air, is more and more widely used for the longterm preservation of food products and biological materials, to operate transport refrigerators, for the needs of cryofracturing of various substances, etc. Various options of hydrogen liqueﬁers (up to 104 l/h), helium liqueﬁers (100 l/h), and refrigerators which reach millikelvin temperatures using 3 He dissolved in superﬂuid 4 He are manufactured. Cryogenic technology applies low-temperature methods to other technical areas, such as superconductivity. Using the phenomenon of superconductivity one may develop economically efﬁcient systems (e.g., large-scale magnetic devices with superconducting magnets for nuclear magnetic resonance imaging, accelerators, and thermonuclear installations). One may attain high speciﬁc power output for electric motors and generators, achieve very high sensitivities in measuring devices using the Josephson effect, etc. Projects are in progress to build superconducting electric power lines and transportation systems. CRYOGENIC TEMPERATURES

Low temperatures, in the range from 120 K to below 1 K (see Low-temperature physics). There exist various methods of deep freezing, or reaching these temperatures: cooling a gas when throttling (Joule–Thompson effect), isoentropic gas expansion in a gas expander, desorption cooling, expansion liquefaction, vapor pumping over a cooling agent, and so on. Combinations of two or more methods are often used. The liquefaction of nitrogen, hydrogen and helium provides the principal refrigerants in technical and scientiﬁc research. Vapor pumping over these liquids produces low temperatures in the range of 120–0.25 K (N2 ∼ 120–63 K; H2 ∼ 20–10 K; 4 He ∼ 4–0.7 K; 3 He ∼ 3–0.25 K). These refrigerants are employed in practice for cooling various electrical engineering devices (superconducting magnets, power transmission lines, electric generators, electric motors, transformers, etc.), electronic devices (radiation detectors, ﬁrst stages of ampliﬁers, computer elements, etc.) and

CRYOSTAT

other units. Deep freezing is used for gas blend separation, gas puriﬁcation, cooling of food, and for other purposes in medicine, construction, engineering, and so on. CRYOSORPTION (fr. Gr. κρυoς , cold, and Lat. sorbeo , absorb)

The process of absorption of gas from the environment by a strongly cooled solid or a cryogenic liquid called a cryosorbent. The removal from the gas phase by the liquid cryosorbent is called absorption. This process is explained by the ﬁnite solubility of certain gases in cryogenic liquids. A solubility coefﬁcient α (in m3 per ton of cryosorbent at 0 ◦ C and 760 mm Hg) is introduced. The value of α is a function of the partial pressure, P , and the amount of the absorbed gas is given by the expression σ = αP . The coefﬁcient α has a different dependence on the temperature for different materials. It decreases with the temperature if gaseous H2 or He is absorbed by liquid nitrogen; while for most gases absorbed by liquid methanol it grows with the drop in temperature. The absorption process is used in several separation cycles. During cryosorption of vapors by porous solids capillary condensation may occur. Cryosorption of vapors from certain multiphase gas systems may proceed by way of freezing the atoms of highly volatile fractions into a solid layer of a weakly volatile fraction precipitated at a cooled surface. A special case of cryosorption is adsorption of a material from the gas phase by a surface layer of a cooled adsorbent. The amount of gas, V , adsorbed by a unit mass of adsorbent depends on the nature of the adsorbent, and that of the adsorbed substance, and it grows for lower temperatures and higher gas pressures. The curve describing the dependence of V on P at T = const is called the adsorption isotherm. The amount of adsorbed gas is linear with pressure at low pressures, following Henry’s law: V = kP . As a rule, several processes proceed in parallel during cryosorption. Cryosorption is widely used in systems of vacuum cryogenic evacuation (see Low-temperature pumping methods).

235

CRYOSTAT (fr. Gr. κρυoς , cold, and σ τ ατ oς , standing, unmoving)

A device for cryostatting, i.e. for maintaining a constant cryogenic temperature between 0 and 120 K. Cryostats are used to study physical properties of materials, the phenomenon of superconductivity, to cool photodetectors, and to pursue other tasks at low temperatures. The simplest cryostat consists of two vacuum concentric bottles. The inner bottle, where the specimen under study is placed, is ﬁlled with a cryogenic liquid boiling at low temperature, e.g., with liquid helium (4.2 K). The outer bottle playing the role of thermal isolation is ﬁlled with a liquid boiling at a higher temperature, e.g., liquid nitrogen (77 K). Cryostats are often used to cool and store the specimen at a speciﬁc temperature within a wide range (from room to a very low value, e.g., 4.2 K). Such a device is not a cryostat in a strict sense, or is not one at every temperature. However, if its minimum attainable temperature falls within the cryogenic range, it is commonly called a cryostat. In most cryostats the sources of cold that absorb the heat removed from the specimen are liqueﬁed gases. The most widely used are liquid nitrogen (N2 ), helium (3 He, 4 He), hydrogen (H2 ) and, less commonly, oxygen (O2 ). Special cryostats used to cool photosensors sometimes contain solid noble gases. More recently compact refrigerators have been developed that can continuously pump a liquid or gaseous cooling agent into a cryostat. Together the two units form a joint cryostatting system. To reach superlow temperatures (T < 1 K) complex multistage devices are employed which achieve cryogenic temperatures of a specimen using liquid gases (3 He–4 He solution refrigerators), or through adiabatic demagnetization (see Adiabatic demagnetization cooling). Depending on the type of study, the cryostat may include optical windows (optical cryostat), a superconducting solenoid, a very high frequency lead, or other devices to probe the specimen in various ways. Many types of cryostats are available, varying in purpose, cooling technique, temperature range covered, permissible thermal load, accuracy, reliability, stability, character of probing, etc. Two main approaches have been followed in building cryostats:

236

CRYOTRON

1. Complex design for highly speciﬁc tasks, e.g., achieving extra low temperatures, cooling superconducting devices, cooling radiation sensors, solving problems in material development, etc. 2. Simple and cheap universal design for scientiﬁc and technological applications, to cover a wide temperature range, have short priming time, quickly reach functional range, have low maintenance cost, match well with peripheral measurement devices, permit manipulation of the cooled specimen, etc. Choosing the technique of heat evacuation from the specimen under study is of particular importance, especially for high heat inﬂux. Several common techniques for heat removal are: thermal radiation exchange, direct mechanical contact with the cooled surface, heat exchange through a gas carrier, the Swenson effect, and forced freezing of a target with a cold gas jet. These are all applicable over a wide temperature range, and have already reached advanced stages of development. The most widely applied cryostats make use of a single cryogenic ﬂuid, and are of two types, namely liquid immersion and stream ﬂow. To absorb thermal energy from the specimen liquid cryostats ordinarily use the heat of evaporation of a liquid coolant, but this only supports a temperature close to the boiling point of the coolant. Over a wide temperature range heat can be absorbed and removed via the speci c heat of a gaseous coolant. The temperature of a ﬂowing gas is easily varied, with the coolant brought directly to the specimen in the amount needed to compensate for the heat input from probing at a given temperature. Stream cryostats are of a more general nature, and permit using all the ﬁve known methods of heat evacuation immediately from the cooled specimen. Stream cryostats have several important advantages over the liquid type: they can achieve any temperature above the boiling point of the coolant; the coolant is very efﬁciently utilized; the temperature can be changed rapidly; the cryostat may be arbitrarily oriented in space; these cryostats are easily made small, etc. This small size capability is particularly important when matching cryostats to standard experimental devices, such as spectral instruments, optical or electronic microscopes, etc.

CRYOTRON

A superconducting device used as a switch, or a memory cell, in computers. Cryotrons employ the phenomenon of superconductivity turn-off by a magnetic ﬁeld. The current in an input circuit magnetically controls the superconductingto-normal transition in one or more output circuits. In practice a cryotron is a superconducting rod, or more commonly, a thin lm which may be in either the normal (switched-off) or superconducting (switched-on) state. A different superconductor with a higher critical ﬁeld controls it. The cryotron is switched from one state to another by varying the current through a control circuit. Cryotrons have the advantage that in their superconducting state the dissipation of energy in them is zero. An important characteristic is the switching time, which in more advanced designs may be as short as 10−10 s. CRYSTAL BASAL PLANE See Basal plane of crystals. CRYSTAL CHEMISTRY Branch of crystallography studying the locations of atoms and particles in crystals, and the nature of their chemical bonds. Crystal chem-

istry brings together the results from experimental X-ray and other diffraction techniques used to study the atomic structure of crystals (see X-ray structure analysis, Electron diffraction analysis, Neutron diffractometry), and combines them with both classical and quantum theories of chemical bonding to compute the energy of crystal structures, taking into account the crystal symmetry. Crystal chemistry approaches make it possible to explain, and in certain cases to predict, the positions of atoms and molecules in a crystal lattice, and their nearest neighbor distances, starting from the chemical composition of the material. Chemical bonding between atoms in crystals results from the interaction between their outer valence electrons. Depending on the nature of the bonding, the equilibrium distance between atoms is usually within 0.15–0.4 nm. When atoms are brought closer together than this a strong repulsion develops. Therefore, to a ﬁrst approximation, certain “sizes” or characteristic radii may be attributed to atoms for each type of bonding. Then

CRYSTAL CHEMISTRY

one may proceed from a physical model of a crystal envisaged as an atomic electron-dominated system, to a geometrical model that looks upon a crystal as an ordered arrangement of incompressible balls. A full crystal chemistry description includes specifying the size of the unit cell, the space group of the crystal, its individual atom coordinates, distances between them, and the types of chemical bonds that are present. In addition, the near environment of separate atoms, the characteristic atomic groupings, thermal vibrations of the atoms, etc., have to be taken into account. In terms of the type of their chemical bonding, crystals may be divided into four major groups: ionic crystals (e.g., NaCl), covalent crystals (e.g., diamond, silicon), metallic crystals (metals and intermetallic compounds), and molecular crystals (e.g., naphthalene). A certain structure is typical for each of these types of crystals. However, when thermodynamic conditions change these may sometimes alter (polymorphism). As a rule, the simpler the chemical formula of the compound, the more symmetric its structure. Crystals with identical chemical formulae (in the ratios of constituent atoms) may have identical crystal structures (identical structural types), despite possible differences in their bonding type (isostructure). Alkali halides of the NaCl type and certain oxides (e.g., MgO), as well as several alloys (e.g., Ti–Ni), are isostructural. Isostructural crystals with the same kind of bonding are called isomorphic (see Isomorphism). In many cases a continuous sequence of solid solutions exists between isomorphic crystals. The geometric model of crystals involves the concept of effective radii of atoms, molecules and ions (crystal chemical radii), so that their bonding distance is equal to the sum of such radii (additivity of crystal chemical radii). Using experimental data one can tabulate crystal chemical radii for all the types of bonding (see Atomic radii, Ionic radius). The principal geometric concept in crystal chemistry is the theory of dense packing that explains the positioning of atoms in certain metallic and ionic structures graphically. For ionic structures one may talk about “holes” in the packing of larger anions that are occupied by smaller cations of similar ionic radii.

237

The structural unit in molecular crystals is a molecule. Crystal chemistry of organic compounds considers the rules of dense packing of molecules, the relation between the symmetry of molecules and the symmetry of the crystal, and the types of organic structures involved. Speciﬁc crystal patterns are identiﬁed in the structures of polymers, liquid crystals, and biological crystals. The coordination number K (see Coordination sphere) and the type of coordination polyhedron characterize the chemical bonding of a given atom, as well as the structure of a given crystal as a whole. For example, Be (with a few exceptions) and Ge form a tetrahedral environment (K = 4), Al and Cr have an octahedron (K = 6) for their coordination polyhedron, and Pd and Pt are often square planar coordinated (K = 4). Low coordination numbers point to a signiﬁcant role of directional covalent bonds, and large K values (e.g., 6, 8, 12) indicate an appreciable role of ionic and metallic bonding. Bonds of various types coexist in many crystal structures (graphite, MoS2 , etc.). Such structures are called heterodesmic structures in contrast to homodesmic ones, the latter featuring uniform bonding (diamond, metals, NaCl, crystals of inert elements), and the former mixed bonding. The laws of thermodynamics determine whether or not a particular crystal structure will form. The structure most stable at a given temperature T is the one that has the lowest Helmholtz free energy F = U − T S, where U is the bonding energy of the crystal (energy needed to break up the crystal into separate atoms or molecules) at T = 0 K, and S is its entropy. The higher the free energy the stronger the bonding in the crystal. It is usually within 40–80 kJ/mol for crystals with covalent bonding, is somewhat lower for the molecular crystals, and is lowest for van der Waals bonding (4–15 kJ/mol). In practice, theoretically calculating the free energy and predicting the structure of crystals is only possible for comparatively simple cases. Such calculations can be carried out within the framework of the band theory of solids. In some cases semiempirical expressions for the potential energy of interaction of atoms in crystals can yield fairly accurate results for certain types of bonding (see Interatomic interaction potentials).

238

CRYSTAL CLASSES

Table 1. Meaning of the ﬁrst (I), second (II) and third (III) terms in the International Symbols of the 32 crystallographic point groups of the seven crystal systems (see ﬁgure). Crystal system

Position of each term in the symbol I

II

III

–

–

–

–

Trigonal

Unit symbol corresponding to any direction Twofold axis and/or reﬂection plane Twofold axis (x) or reﬂection plane Threefold symmetry axis

Hexagonal

Sixfold symmetry axis

Tetragonal

Fourfold symmetry axis

Cubic (isometric)

A symmetry element

Triclinic Monoclinic Orthorhombic

CRYSTAL CLASSES

Crystallographic classes or symmetry classes are categories of crystallographic point groups of symmetry (introduced in 1830 by J. Hessel and, independently, by A.V. Gadolin in 1867). To denote crystal classes symbols are used (see Crystal symmetry) that are based on group theory theorems for the combination of symmetry operations. According to these, the product of two symmetry elements produces another element of the symmetry group. Table 1 presents notational rules for crystal classes that are found in various crystallographic systems. For example, the point group 43m corresponding to the mirror plane class of the cubic system, denoted by Td (dihedral-tetrahedral) in the Schönﬂies system, has a fourfold inversion axis (4), a threefold rotation axis (3) and a mirror plane (m). The axial monoclinic point group (Schönﬂies C2 ) has only a twofold axis. The coordinate and diagonal elements of symmetry are understood as planes and axes passing along the coordinate planes (axes) and the bisectors of the angles between them, respectively. The crystal classes are separated into primitive (single symmetry axis), centric (symmetry axis plus center of symmetry), planar (n symmetry planes along the axis), axial (having n twofold axes normal to the symmetry axis), etc. Elements of the crystal

Twofold axis (y) or reﬂection plane Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane Diagonal threefold axis

Twofold axis (z) or reﬂection plane – Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane

classes of the 32 crystallographic point groups are presented in the ﬁgure. CRYSTAL CLEAVAGE The capacity of monocrystals to be split

(cleaved) along certain crystallographic planes (crystal cleavage planes) on exposure to a mechanical force or impact. The cleavage is related to the speciﬁc features of the crystal structure. The crystal is split along directions or planes of smallest crystallographic indices, which involves the breakage of the weakest bonds. Thus, the graphite structure is susceptible to actions counteracting van der Waals forces perpendicular to (0001), which involves the separation of adjacent sheets of carbon atoms from one another. Most cubic crystals cleave along cubic planes. The crystal cleavage plane of BCC metals is often (100), whereas hexagonal crystals cleave along the basal plane. The orientation of the cleavage planes of certain crystalline materials (e.g., sphalerite) is determined by the charge of adjacent separable atomic sheets. Cleavage along planes of opposite charge requires more energy than splitting along planes containing ions of the same sign. The following degrees of cleavage of crystals are distinguished: highly perfect cleavage (cleaved into thinnest layers), perfect cleavage (crystal split

CRYSTAL DETECTOR

into bars along cleavage plane), average degree of cleavage (cleavage facets accompanied by randomly shaped facets), imperfect cleavage (fractography patterns exhibit mostly macroscopically irrational fracture regions), completely imperfect cleavage (practically no cleavage: fracture is conchoidal). Cleavage is one of the characteristic properties of a crystalline material. It is helpful for the determination of a crystal disorientation. Surfaces of high perfection, exposed on splitting along the crystal cleavage plane, are convenient for study. The phenomenon of crystal cleavage is used in jewelry trades to prepare a gem for its crystal faceting.

239

CRYSTAL DETECTOR, crystal counter

An instrument to record and analyze spectroscopic properties of nuclear particles and photons. The crystal counter is an electric capacitor (usually parallel plate type), ﬁlled with a single crystal insulator (e.g., diamond or CdS). A charged particle entering the dielectric produces ionization along its path, and free current carriers appear which are driven to the capacitor electrodes by the external electric ﬁeld. A short electric pulse results, its amplitude proportional to the energy released by the particle in the crystal. After ampliﬁcation it is recorded by a counting device or amplitude analyzer.

240

CRYSTAL DIFFRACTION SPECTROMETERS

Simplicity of design and maintenance, small size (below 1 mm2 ) and the fact that certain crystals, e.g., diamond, can function at high temperatures, make crystal counters convenient nuclear radiation detectors that are widely used in physics, dosimetry, various industrial applications, etc. CRYSTAL DIFFRACTION SPECTROMETERS

A class of X-ray spectral instruments for studying absorption and emission spectra of matter and the structural features of monocrystals. Crystal diffraction spectrometers may be single-axis (sample crystal), double-axis (collimator crystal plus sample), and triple-axis (collimator, sample, and analyzer crystals) types. As the number of elements in the instrument grows, its spectral dispersion and angular divergence of the radiation diminish, so that it becomes possible to better expand the diffracted intensity over the angle. Single-axis diffraction spectrometers are only capable of measuring the integrated intensity of the diffraction. Double-axis instruments can record X-ray spectra or rocking curves for monochromatic radiation (i.e. dependence of diffracted intensity on X-ray angle of incidence). They also provide for antiparallel and parallel positioning of the crystals so that the resulting dispersion is either doubled after the beam passes through the sample crystal, or it reverts to zero. The ﬁrst position is used for spectral studies, and the second (zero dispersion) for structural studies during which the width and intensity of the diffraction maximum are measured. Triple-axis spectrometers permit the separation of the coherent component of the integrated intensity from the diffuse one. See also X-ray spectrometer. CRYSTAL FACETING, crystal cut

Outward shape of crystals speciﬁc for a given crystal class. Faceting conforms strictly to the

point group symmetry relationships of a crystal (see Crystal symmetry), and only includes faces of certain categories, the so-called simple forms (see Crystal polyhedron). As a rule, the simple forms that are possible within a given point group symmetry tend to display various combinations one with another. The shapes of individual crystals are closely related to their structure. Materials without

clearly preferred directions form, as a rule, uniformly developed isometric polyhedra. The acicular crystals are typical of materials with needlelike or chain structures; plate-like crystals are typical of materials with laminated structures, and so on. In most cases, the only crystal faces that participate in the crystal faceting are those parallel to crystal lattice planes of the structure. The latter possesses high reticular density, i.e. their unit area maximizes the number of particles (Bravais law). In an ideal case the faces of each simple form must have the same conﬁguration and dimensions. The shape of a real individual crystal is determined by the speciﬁc conditions of its growth: temperature, pressure, concentration, impurity atoms content, etc. When characterizing the crystal faceting, the terms form and habit are commonly used. The former term concerns a general view of a polyhedron (isometric, acicular, ﬁbriform, etc.), while the latter serves to describe the outward appearance of the individual crystal with the help of dominant simple forms (octahedral, prismatic, dipyramidal, and so on). CRYSTAL FIELD, internal crystal eld, crystalline electric eld The electric ﬁeld at a point within a crystal,

produced by its atoms or ions. This ﬁeld determines energy level splittings of atomic electronic conﬁgurations, and the periodic potential of the crystal ﬁeld determines the band structure of the crystal for an ideal lattice corresponding to the crystallographic space group. An impurity ion (or local ionic center) has an energy spectrum determined by the local crystal ﬁeld symmetry. The internal electric ﬁelds of defects bring about an inhomogeneous broadening of the spectral lines of resonant transitions. The line shape (proﬁle) depends on the nature of the defects and their distribution within the crystal. To compute the shape of the resonance lines one can use statistical theory of line shape, or possibly the method of moments. Crystal eld theory is applied in various branches of physical science (optics, radiospectroscopy, etc.) to calculate the energy transitions responsible for spectra. It considers various models of the ﬁeld, and basically accounts for the spatial motions of electrons and nuclei. Energy level splittings produced by the crystal ﬁeld generally

CRYSTAL FIELD THEORY

lie in the optical frequency range (1013 –1015 Hz). Accounting for the spin variables along with the spatial degrees of freedom results in an additional splitting or shifting of the levels. The crystal ﬁeld affects the spin through the spin–orbit interaction. Spin level splittings may be treated using a framework similar to crystal ﬁeld theory called the spin Hamiltonian technique. The energy level spacings associated with electron spin interactions lie in the frequency bands of electron paramagnetic resonance (108 –1011 Hz), while those resulting from the nuclear spin are 2 to 3 orders of magnitude smaller, the same as the frequency range of nuclear magnetic resonance. CRYSTAL FIELD GRADIENT

A symmetric second-rank zero trace tensor with components equal to the second derivatives of the potential V (r) of the electric ﬁeld at the site of an atom or ion in a crystal: Vαβ = (∂ 2 V /∂xα ∂xβ )|r=0 . The crystal ﬁeld gradient deﬁnes the energy H of the quadrupole moment Qαβ of a nucleus (see Quadrupole), located at the site: (2) Qαβ Vαβ = Qm V−m , H= αβ

m

(2)

where Qm are the components of the tensor operator of the nuclear quadrupole moment: 1 Vzz , 2 1/2 1 V±1 = ± (Vxz ± iVyz ), 6 1/2 1 V±2 = (Vxx − Vyy ± 2iVxy ). 24 V0 =

The crystal ﬁeld gradient of the tensor Vαβ in a system with two principal axes is characterized by two independent parameters eq = Vzz and η = (Vxx − Vyy )/Vzz , where |Vzz | |Vyy | |Vxx |, the dimensionless asymmetry parameter η is limited to the range 0 η 1, and the Hamiltonian of the quadrupole interaction assumes the form −1 H = e2 qQ 4I (2I − 1) × 3Iz2 − I (I + 1) + η Ix2 − Iy2 ,

241

where q is the quadrupole moment of the nucleus with a spin I 1. The crystal ﬁeld gradient for cubic symmetry is zero. When calculating a crystal ﬁeld gradient one has to take into consideration the ﬁelds of point charges (lattice summation carried out by the Ewald method), and the multipole moments of ions and conduction electrons. To take into account the polarization of the full electron shells of an ion in the crystal e ld, its ﬁeld gradient at the nucleus is written in the form (1 − γ )Vαβ , where γ is the antiscreening factor. For most ions the value of γ is within the range from −10 to −100. CRYSTAL FIELD SPLITTING See Bethe splitting. CRYSTAL FIELD THEORY (H. Bethe, 1929) Theory describing electronic states of ions with unﬁlled d- and f -shells in crystals. The scope

involves such areas as optical spectroscopy, magnetic properties, and mechanisms of the electron– phonon interaction, in crystals containing ions of the three transition metal groups, the lanthanides, and the actinides. Crystal ﬁeld theory treats the splitting of electronic energy levels of localized dand f -electrons by an effective internal crystalline ﬁeld. The Hamiltonian is solved using perturbation techniques for a single conﬁguration, with the states of a single electron in the central ﬁeld of a free ion taken as the zero-order approximation. The perturbation operator deﬁned in the space of the wave functions of the (nl)N -shell equals the sum of the energies of the electrostatic interaction, Hee , the spin–orbit interaction, H so , and the energy of the electron in the crystal ﬁeld, Hc . The Hamiltonian, Hc is averaged over the radial distribution of electron density, and has the form: Hc =

N i

(k)

(k)

Bqk Cq (i),

kq

where Cq (i) are spherical operators in the space of angular variables of the ith nl-electron, and Bqk are the crystal ﬁeld parameters, quantitative characteristics of the potential of the electric ﬁeld at the paramagnetic ion site in an equilibrium conﬁguration. They have dimensions of energy, are generally complex, and satisfy the relations

242

CRYSTAL FIELD THEORY

k . The number of independent Bqk ∗ = (−1)q B−q parameters depends on the symmetry of the crystal ﬁeld, while the structure of the operator Hc is determined by the choice of local coordinate system. For example, a cubic crystal ﬁeld has the octahedral point group of symmetry Oh . In the system of Cartesian coordinate axes coinciding with the C4 symmetry axes the Hamiltonian of the electron interaction with the cubic crystal ﬁeld is given by 5 (4) (4) (4) C + C−4 H = B4 C 0 + 14 4 7 (6) (6) (6) + B6 C 0 + C4 + C−4 . 2

The even component of the crystal ﬁeld potential is the same in the case of tetrahedral (Th , Td ) coordination. Often the cubic symmetry component dominates at a low-symmetry site. The parameter 10Dq = (10/21)B4 equals the difference between the two d-electron energies in a crystal ﬁeld of cubic symmetry (doublet eg and triplet t2g states), and provides a measure of the ﬁeld “strength” for ions with partially ﬁlled d n -shells. The f n -shell multiplet splittings in cubic symmetry are deﬁned by the parameters B4 and B6 , and the structure of the wave functions of the respective states depends on only a single parameter (x), proportional to the ratio B4 /B6 . The effects produced by the spatial correlation of electrons, and the change of the electrostatic interaction parameters in the crystal ﬁeld, are described by a two-term operator: (k) (k k )k (2) C (k1 ) (i) × C (k2 ) (j ) Bq Bq 1 2 , Hc i>j

that has a complex tensor structure. The parame(k k )k ters Bqk , Bq 1 2 can be evaluated from optical or magnetic measurements, or computed within various crystal ﬁeld models. Quantum-mechanical calculations taking into account the electron structure of the nearest neighbors of a paramagnetic ion are sometimes called ligand ﬁeld theory. When calculating the energy spectrum of the (nl)N electron shell one should distinguish between strong crystal ﬁelds (ions of 4d and 5d transition groups, Hc > Hee > Hso ), intermediate ﬁelds (ions of the 3d iron group, Hc ∼ Hee > Hso ), average ﬁelds (Hee > Hc > Hso ), and weak ﬁelds (rareearth elements, Hee > Hso > Hc ). Various options

for constructing the matrix of the Hc operator depend on the choice of the basis for the zeroth approximation (e.g., single electron wave functions, functions of terms |γ LSML MS , or functions of multiplets |γ LSJ MJ ). Piezospectroscopic or electric ﬁeld effects in the spectra of paramagnetic crystals can result from changes in the crystal ﬁeld during corresponding external actions on the lattice. Modulation of the crystal ﬁeld by lattice vibrations is the principal mechanism of the electron–phonon interaction. Crystal ﬁeld models help with computational techniques. The simplest and historically the ﬁrst point charge model envisaged the crystal lattice as a collection of point charges Qλ e located at lattice sites (λ labels the site), with the charges themselves prescribed by the valences of the respective ions. To determine the ﬁeld of point charges one has to calculate the lattice sums: 1/2 4π k q e2 r k Bq = −(−1) 2k + 1 ×

k (θ ϕ ) Qλ Y−q λ λ λ

Rλk+1

,

where Yqk are spherical harmonics, rλ , θλ , ϕλ are the spherical coordinates of site λ (the paramagnetic ion is at the coordinate origin), and r k are the moments of the electron radial density in the unﬁlled shell. Discrepancies of an order of magnitude often exist between calculated and measured crystal ﬁeld parameters. To account for this one may consider changes in the radial density of the d- and f -electrons in the crystal ﬁeld, ﬁelds of point multipole moments (dipoles, quadrupoles), the distribution of charges of lattice ions, screening of f -electrons by the outer ﬁlled electron shells, etc. The electronic structure of selected complexes that include the paramagnetic ion and its nearest neighbors (ligands) immersed in the crystal is treated by cluster models (see Cluster). Electron energies in the complex are calculated using a one-electron Hamiltonian that operates in the space of molecular orbitals (LCAO method, see Molecular orbital), or in the space of mixed conﬁgurations. Charge transfer from the ligands to the paramagnetic ion is also taken into account (the Heitler–London approximation). To

CRYSTAL LATTICE

simplify estimates of matrix elements of the oneelectron Hamiltonian (see Single-electron approximation) one uses either the Mulliken–Wolfsberg– Helmholtz method (R.S. Mulliken, M. Wolfsberg, G. Helmholtz, 1952) or the local exchange potential (Xα -technique). The dominant role in forming the energy spectrum of the cluster and the corresponding potential of the effective crystal ﬁeld involves effects produced by the overlapping of the spatial distributions of charges of the ligands and the paramagnetic ion. Among such effects are the Kleiner correction to the Coulomb ﬁeld of the ligands, the exchange interaction, the mutual nonorthogonality of wave functions of the ligands and the metal ion, covalency, virtual excitations of the cluster accompanied by charge transfer from the ligands to the paramagnetic ion, followed by the formation of holes in its ﬁlled electronic shells. One may explicitly determine the interrelations between the composition and structure of the crystal lattice, on the one hand, and the energy spectrum of the paramagnetic ions on the other, using semiphenomenological models that involve a limited number of parameters determined from experimental data. The energy of an nl-electron in an axially symmetric ﬁeld of the ligand λ is

k (k) equal to Hc(λ) = k B 0 (Rλ )C0 (quantization axis parallel to r λ ). Assuming that individual ligand ﬁelds may be summed, and using the power k −t series approximation B 0 ∝ Rλ k , one may express the terms of the crystal ﬁeld through four (k = 2, 4 for l = 2) or six (k = 2, 4, 6 for l = 3) parameters of the “superposition model” k B 0 , tk . To parameterize the spectra of paramagnetic ions using the model of angular overlap and the model of exchange charges it is sufﬁcient to k represent the functions B 0 (Rλ ) by linear combinations of squared overlap integrals of the wave functions of the d- (or f -) electron with the ligand wave functions. Satisfactory models are still lacking for rare-earth metals and actinide compounds. The so-called odd components of the crystal ﬁeld are treated separately since they mix together the states of different parity that correspond to the ground state ((nl)N , 1 = N < 2(2l + 1)), and to the excited ((n l )4l +1 (nl)N+1 , (nl)N−1 (n l )) electronic con gurations of the ions of rare-earth and transition metals. The energy of a localized

243

electron in an odd crystalline ﬁeld corresponds

2p+1 2p+1 to the Hamiltonian H = Bk Ck , deﬁned in the subspaces of one-electron functions 2p+1 n l ml |, |nlml with their parameters Bk (where 0 p (l + l − 1)/2) different from zero when the point group of symmetry of the ion does not include inversion. The odd components control the intensities of the dipole transitions between the states of an unﬁlled (nl)N -shell (forbidden for free atoms), as well as the linear electric eld effects in optical spectra and the spectra of paramagnetic crystals. When perturbation theory is applicable one can introduce an effective operator (H A + AH )/Δ instead of the odd single particle operator A in the space of states of the basic electron conﬁguration. Here Δ is the average energy difference between the excited and ground state conﬁgurations. Additional terms in the effective operator of the dipole moment proportional to the squared electron radius (r 2 ) are called pseudo-quadrupole moments. Calculating the Stark structure of the spectrum of the unﬁlled shell, the effective even ﬁeld H 2 /Δ is allowed along with the even component of the crystal ﬁeld. The odd components, induced by odd vibrations, deﬁne the intensities of the electron– vibrational transitions between the states of the same parity for ions in the crystal lattice sites, the latter also serving as the centers of symmetry. CRYSTAL GRAINS See Polycrystal. CRYSTAL, IDEAL See Ideal crystal, Perfect crystal. CRYSTAL LATTICE

A geometrically ordered arrangement of atoms (ions, molecules) typical of the crystalline state of matter (see also Lattice). The geometry of an ideal crystal involves a spatial periodicity (translational symmetry, see Crystal symmetry) characterized by three noncoplanar basis vectors a j (j = 1, 2, 3) such that the displacement of the lattice by a vector n1 a 1 + n2 a 2 + n3 a 3 (n1 , n2 , n3 are integers) brings it into itself. If every a j is selected to be the shortest possible displacement in its respective direction, the parallelepiped formed by the three

244

CRYSTAL LATTICE BASIS

basis vectors is called the unit cell or the primitive parallelepiped. By simply replicating the unit cell in space one may generate the entire crystal structure. The choice of the set of a j vectors is not unique; yet the unit cell volume is independent of such a choice. If a unit cell can be chosen so that it contains only a single atom then it is called a primitive cell. All other unit cells are called nonprimitive cells. A complex crystal lattice may be envisaged to consist of one or several Bravais lattices ﬁtted into each other, each such Bravais lattice being built of atoms of a single type. The presence of a crystal lattice explains the phenomenon of anisotropy of crystals and crystal faceting. Experimentally, crystal lattices can be identiﬁed and classiﬁed by X-ray, electron, and neutron diffraction techniques. CRYSTAL LATTICE BASIS, unit cell basis

Set of atoms and their coordinates with the same location at each point of a Bravais lattice. By adding the basis to the Bravais lattice, one obtains a crystal lattice structure. CRYSTAL LATTICE CONSTANTS

The magnitudes of three noncoplanar translations (a, b, c), by which the Bravais lattice may be constructed for a given crystal. The lattice is to satisfy three main conditions: (1) the symmetry of the lattice unit cell must correspond to the microscopic crystal symmetry; (2) the unit cell is to possess the highest possible number of right angles (or the highest possible number of equal angles and equal sides); (3) the unit cell is to have a minimal possible volume (with due regard for the conditions (1) and (2)). The set of crystal lattice constants (a, b, c) and the angles between them: α (between b and c), β (between a and c) and γ (between a and b), is called the crystallographic basis. There are seven types of crystallographic basis sets that correspond to the seven crystallographic systems, as follows: • a = b = c, α = β = γ = 90◦ , cubic system; • a = b = c, α = β = γ = 90◦ , tetragonal system; • a = b = c, α = β = 90◦ , γ = 120◦ , hexagonal system; • a = b = c, α = β = γ = 90◦ , trigonal system;

• a = b = c, α = β = γ = 90◦ , orthorhombic system; • a = b = c, α = β = 90◦ , γ = 90◦ , monoclinic system; and • a = b = c, α = β = γ , triclinic system. CRYSTAL LATTICE DYNAMICS

The branch of solid-state mechanics, which studies the internal movements within a crystal, taking into account the discreteness of its atomic structure. It includes the classical and quantum mechanics of collective movements of atoms in an ideal crystal, the theory of interactions of the crystal with penetrating radiation, and also the dynamics of imperfect crystals. Due to the strong chemical bonding the internal motion cannot be described as the superposition of independent displacements of separate atoms. If the displacements are small and the harmonic approximation applies then normal vibrations occur, each of which involves the participation of all the atoms. The normal vibration has a form of a plane wave characterized by the wave vector k, expressed within the ﬁrst Brillouin zone, which determines the direction of propagation of the wave front, with wave length λ = 2π/|k|, and a polarization vector which indicates the direction of the displacement of atoms within the wave. During the course of a normal vibration all the atoms of the crystal vibrate harmonically near their equilibrium positions at the same frequency ω which is determined by the dispersion law that connects the values of ω and k: ω2 = fα (k),

α = 1, 2, . . . , 3q,

where α denotes the branch of the dispersion law and q is the number of atoms in the crystallographic unit cell. In three dimensions there are at least three branches of vibrations. In the long-wave approximation (λ a, a is the interatomic distance) all the atoms in the unit cell vibrate with the same phase, corresponding to acoustic vibrations (Fig. 1(a)). In this limit λ a they are transformed into the usual sound waves in a solid with the linear dispersion law ω = cs k, s = 1, 2, 3. Acoustic vibrations cover the frequency band from 0 to 1013 Hz. At high frequencies the dispersion law is no longer linear. However, in the

CRYSTAL LATTICE DYNAMICS

245

Fig. 1. Diagram of a long-wave vibration of a one-dimensional crystal: (a) acoustic mode; (b) optical mode.

Debye model it is assumed that acoustic vibrations satisfy the linear dispersion law at all frequencies within the range 0 < ω < ωD , where the Debye frequency ωD is the maximum possible vibrational frequency (1013 Hz), and serves as the most important parameter of the spectrum of crystal vibrations. In a complex crystal lattice (q > 1), 3q − 3 branches of optical vibrations are possible, and at k = 0 the center of mass of the unit cell remains stationary with the motion reduced to relative displacements of atoms within the unit cell (Fig. 1(b)). In the limit k → 0 the optical vibration frequencies ω(0) are different from zero. Ordinarily the frequency bands of optical vibrations are located above those of acoustic vibrations, with a forbidden region, or band gap, separating them. It is also possible for acoustic and optical frequency bands to overlap. There are crystals in which some optical frequencies strongly depend on external parameters (temperature, pressure, magnetic ﬁeld, etc.) and at speciﬁc values of these parameters they may tend to zero (soft modes). As a result, static relative displacements of atoms can occur, i.e. the unit cell is restructured by undergoing a structural phase transition. Optical vibrations of ionic crystals can strongly interact with an electromagnetic ﬁeld producing coupled polarized vibrations of the lattice and the ﬁeld. This phenomenon permits the excitation of optical vibrations of ionic crystals by incident oscillating electromagnetic ﬁelds (e.g., light waves), generally in the IR frequency range, which is the reason for calling these frequencies optical.

Many lattice modes can be excited simultaneously with different amplitudes. The total number of possible independent vibrations equals the number of mechanical degrees of freedom of all the atoms in the crystal, and their distribution in frequency is determined by the frequency distribution function ν(ω) (phonon density of states). The form of ν(ω) strongly depends on the dimensionality of the crystal. In a three-dimensional lattice at low frequencies (ω ωD ) for each acoustic branch ν3 (ω) ∝ ω2 /ωD 3 . For increasing frequency the behavior of ν(ω) changes: it tends to zero at the band edges, and within the bands it exhibits Van Hove singularities (Fig. 2). The overall vibrational density of states is obtained by summing the distributions of the individual branches. The quantum dynamics of a crystal lattice is well described by the harmonic approximation: to each wave of normal vibration with frequency ω and wave vector k there is a corresponding quasi-particle with the energy ε = ω and quasi-momentum p = k, with the number of quasi-particles proportional to the wave intensity. These quasi-particles are the elementary excitations of crystals and are called phonons; they obey Bose–Einstein statistics and form an ideal gas in the harmonic approximation. At sufﬁciently low temperatures when the crystal is weakly excited mechanically, its thermodynamic properties arise from these elementary excitations, and in particular the lattice portion of the crystal energy coincides with energy of the phonon gas. The quantum nature of the crystal motions is manifested through the presence of so-called

246

CRYSTAL LATTICE VIBRATIONS

(1)

Fig. 2. Plot of the frequency distribution function in a three-dimensional crystal for the acoustic (0 < ω < ωm ) and (2) (3) optical (ωm < ω < ωm ) branches, where ω1 , ω2 , ω3 , ω4 are the frequencies of Van Hove singularities.

zero-point vibrations of atoms at T = 0 K. The amplitude of these vibrations is usually considerably smaller than the interatomic distance, but in crystals consisting of light atoms it may not be so very much smaller (quantum crystals He, H2 , Ar). In solid He the zero-point vibrations are so pronounced that the solid state exists at T = 0 K only under a pressure of more than 25 atm. At lower pressures it “melts” and transforms into a quantum liquid. Other crystals simply melt with an increase in temperature. Melting involves the disruption of the crystal structure and the long-range order, and it occurs when the average amplitude of vibrations of atoms exceeds some critical value. With increasing amplitudes of vibration, anharmonic behavior begins to appear. Anharmonic vibrations cause interactions of phonons and play an important role in kinetic processes such as thermal conductivity and sound absorption in crystals. The interaction of phonons with other elementary excitations (electrons, excitons, spin waves) inﬂuences the dynamics of the crystal lattice through the electrical conductivity, and the optical and relaxational properties of the crystals. The dynamic interaction of a crystal with photons (including X-rays and γ -quanta), neutrons and accelerated charged particles not only reﬂects the structural features of the crystalline state, but also provides experimental methods for investigating the dynamics of crystal lattices. For example, inelastic neutron scattering can furnish the dispersion law and polarization of the vibrations; and the Mössbauer effect can provide estimates of the rootmean-square displacements of vibrating atoms.

CRYSTAL LATTICE VIBRATIONS

Coherent oscillatory motion associated with a crystal lattice. The theory of crystal lattice vi-

brations uses the Born–Oppenheimer adiabatic approximation (M. Born and R. Oppenheimer, 1927), whereby the relatively light and fast moving electrons adiabatically follow the relatively slow motion of heavy atomic nuclei or ions. This justiﬁes presenting the potential energy of a crystal as a function of atomic coordinates only. Assuming small vibrational amplitudes, the potential energy is expanded in a power series in the displacements of atoms from their equilibrium positions. Taking into account only quadratic terms of the expansion corresponds to the harmonic approximation, and leads to linear equations of motion. If us (n) is the displacement of the sth atom in the unit cell of vector-number n, its variation with time is given by the equation: ms d2 uls (n) ik + βss (n, n )uks (n ) = 0, dt 2 nsk

where ms is the mass of the sth type of atom, i and ik (n, n ) are force k are Cartesian indices, and βss constants. Normal vibrations emerge as eigensolutions of the lattice vibration equations. There are 3 acoustic vibration modes and 3q − 9 optical vibration modes for q > 3 (q is the number of atoms in the crystallographic unit cell). Thus the superconductor Tl2 Ba2 CaCu2 O8 has 3 acoustic modes and 36 optical modes of vibrations (16 Raman active and 20 infrared active). CRYSTALLINE STATE, GASEOUS See Gaseous crystalline state.

CRYSTALLIZATION

CRYSTALLITE, MICROSee Microcrystallites. CRYSTALLITES

Small crystal grains (see Polycrystal) in various polycrystalline formations: metal ingots, processed metals and alloys, rocks, minerals, ceramics. Fine monocrystals lacking a clear crystallographic polyhedral shape, and large microcrystals with poorly developed structure (dendrites), plastic deformed microcrystals, etc., are also called crystallites. Depending on the nature and conditions of formation, the average size of crystallites varies within the limits 5–10 μm, with their orientation either arbitrary or following certain patterns (textures). As far as their shape is concerned, crystallites may be equiaxial, columnar, platelike, etc. The crystallite structure strongly affects the strength, plasticity, and other properties of a substance as a whole. Quenching the liquid phase yields particularly ﬁne crystallites, down to the so-called X-ray amorphous structure range (crystallites below 3 nm in size). CRYSTALLIZATION

The process of transforming a substance from its liquid, amorphous or gaseous phase into a crystal. For a crystal to form it is necessary for the chemical potential μ of the crystal phase (which depends on pressure p, temperature T , and concentration c) to be lower than the respective chemical potential of the initial phase. Since a crystal phase usually corresponds to lower temperatures, higher pressures and concentrations in the phase diagram than those found at the point of phase equilibrium, one needs to produce overcooling T , excess pressure p, or supersaturation

c in the initial phase. The relation between

T , p, c and the change in chemical potential, μ, may be expressed as

T , T

p

μ = kB T , p

μ = H

(1)

c , c where H is the change in enthalpy per particle during the phase transition, and k B is the Boltzmann constant.

μ = kB T

247

Crystallization may occur via random formation and growth of crystal precipates (embryos) in various parts of the total volume of the initial phase, a process called mass crystallization. During the formation of a precipitate the binding energy of particles entering it (either atoms or molecules) is released. Energy is expended to form the precipitate surface. For a spherical precipitate of radius r the total change of thermodynamic potential is w(r) = −

4π 3 μ r + 4πr 2 α, 3 v

(2)

where v is the volume per individual atom or molecule, and α is the interphase energy per unit surface area of the precipitate (coefﬁcient of surface tension). The function w(r) is nonmonotonic, and reaches a maximum at r = 2αv/ μ. The corresponding radius of the precipitate is called the critical radius r c , and the energy of its formation is w(rc ) = (16π/3)(α 3 v 2 / μ2 ). Precipitates of a critical radius (see Critical embryos) are in a state of unstable equilibrium with their environment. An increase or decrease of the precipitate radius results in its growth or decay, respectively. When a precipitate forms in an initial phase containing no extraneous microimpurities, the process of its formation is called homogeneous precipitation. When the initial phase contains microimpurities, critical precipitates may form at their surface (or on the walls of the container). In that case, the formation process is called heterogeneous precipitation. The ratio between the work required to form precipitates of a critical radius heterogeneously and homogeneously is given by 1 ψ(θ) = (1 − cos θ)2 (2 + cos θ), 4

(3)

where θ is the edge angle depending on the coefﬁcient of surface tension at the system interfaces. These are the initial phase–microimpurity; microimpurity–crystal; and crystal–initial phase interfaces. Wetting lowers the work of precipitate formation. The number of precipitates of a critical radius per unit volume of the initial phase is proportional to the probability of their formation: exp[−w(rc )/(k B T )]. The respective proportionality coefﬁcient is close to the number of molecules

248

CRYSTALLIZATION CENTER

in a unit volume, n. The rate of formation of precipitates I , i.e. the number of precipitates formed in a unit volume per unit time, may be determined within the formalism of the thermodynamic theory of their formation. One has to multiply the density of precipitates of a critical radius by the number of atoms (molecules) striking their surface per unit time: ⎧ 4πrc2 pn(2πmk B T )−1/2 , ⎪ ⎪ ⎪ ⎪ ⎨ precipitatesform from gas phase, E I= 2 , 4πrc nνa exp − ⎪ ⎪ ⎪ kBT ⎪ ⎩ precipitates form from condensed phase, where m is the mass of the molecule, a is the atomto-atom distance, ν is the frequency of atomic oscillations, and E is the activation energy for particles adding to the precipitate. To account for the evolution of the system of precipitates of radii below rc in the initial phase one adds an extra term in the expression for I , namely: 4rc α 1/2 , z= 9k B T nc where nc is the number of particles in a precipitate of a critical radius. With decreasing temperature (at relatively small overcooling) I grows as precipitates grow, since their formation energy diminishes; on the other hand, the energy of thermal motion and the mobility of particles in the initial phase simultaneously decrease, so that the rate at which they add to the surface of the precipitate decreases as well. Competition between these two factors produces a maximum of I at a certain temperature, after which it starts to decrease at lower temperatures. The value of I is remains negligibly small at comparatively small supercooling (or supersaturating) of the initial phase, so that very few precipitates form in volumes of appreciable size. In other words, the initial phase remains in a metastable state. The range of respective supercooling (supersaturating) is called the metastability range. As a result of the mass crystallization a polycrystal forms, with ﬁne crystals growing from separate precipitates (crystallites) that ﬁll the volume of the initial phase with their crystallographic axes randomly oriented. The structure of the polycrystal depends on the values of I and v. Its

granularity roughens for larger I and smaller v. See also Monocrystal growth. CRYSTALLIZATION CENTER See Crystal nuclei. CRYSTALLIZATION FROM THE GAS (VAPOR) PHASE The formation of crystals by the transformation

of a material from its gas (vapor) phase to a solid. When crystals grow from the vapor an adsorption layer differing from the crystal in composition and properties appears at the crystal–medium interface (see Adsorption). Moreover, surface diffusion of the adsorbed particles at the growing faces plays a decisive role there. Crystallization from the gas phase has been used to produce massive monocrystals, plates, bands, acicular crystals, thread-like crystals, and epitaxial lm s. Condensation techniques and chemical reactions are also employed to grow crystals. When using the ﬁrst it is assumed that material reaches the growing crystal as an atomic or molecular vapor, or as associations of such particles. Depending on the technique used to bring the material to the crystallization zone one may speak about molecular beams in vacuo (see Molecular beam epitaxy), cathode sputtering (see Sputtering), volume vapor phase in an isolated system, and crystallization in an inertial gas ﬂow. To obtain high quality crystals and ﬁlms chemical reaction techniques (e.g., as chemical transport, decomposition of compounds, chemical synthesis in the vapor phase) appear to be quite efﬁcient. In certain cases when ﬁlaments or massive crystals are grown (as well as epitaxial ﬁlms), the vapor–liquid–crystal transport mechanism is employed. Vapor material reaches the growing crystal through a liquid layer of different composition formed either unintentionally or intentionally on the growing surface by introducing impurities into the crystallization zone. It may result from deviations from a stoichiometric composition, or present a liquid phase intentionally formed at the substrate as a smelt droplet of a prescribed composition. The phase-to-phase energy of the crystal–vapor interface is almost an order of magnitude less than the respective energy of the crystal–vapor interface. Two-dimensional precipitates (embryos)

CRYSTALLOGRAPHIC INDICES

form at the liquid–crystal interface at a rate that is much higher than such a rate at the vapor–crystal interface. This feature combines with other factors (such as a higher condensation coefﬁcient at the liquid surface, low resistance to diffusion in the smelted droplets, etc.) to sharply increase the growth rates. CRYSTALLIZATION, HYDROTHERMAL See Hydrothermal crystallization. CRYSTALLIZATION OF POLYMERS First-order phase transition in polymeric systems. Crystallization of high molecular weight

polymers is more complex than crystallization of low molecular weight substances because of the inﬂuences of various parts of the polymer chains (main chain links and side branches). Long chain polymers have a primary structure from the linking together of their repeat units or monomers. A secondary structure can arise from coiling or linking nearby parts through weaker hydrogen bonds, and a tertiary structure can form if larger sections fold into themselves to form a globular or condensed conformation. A crystal structure can form from stretched out and aligned macromolecular chains, from regularly arranged molecular chains folded “upon themselves”, from adjacent polymers interlinked in a quaternary structure, etc. These various conformations of the macromolecule as a whole are found in a crystal with unchanged sublattice parameters (repeatedly packed chain links or monomers), and an unchanged translation period along the primary chain axis. There are globular crystals, supercrystals, with long-range ordering in the packing of the macromolecules (see Long-range and short-range order), e.g., globular proteins or their elements (blocks, co-polar blocks). Such longer range ordering may be present along with short range ordering in the packing of repeated molecular chain links. Deformation processes affecting the conformations of macromolecules can affect the ability of some polymers to crystallize (polyisobutylene is an example). CRYSTALLIZATION, SELF-SUSTAINING See Self-sustaining crystallization.

249

CRYSTALLIZATION WAVES

A particular form of slowly damping oscillations of the interface between solid and liquid helium at low temperatures (below the lambda point 2.17 K) where liquid 4 He is a superﬂuid quantum liquid (see Super uidity) and solid 4 He is a quantum crystal. When a crystallization wave propagates through this system it is accompanied by periodically alternating melting and crystallization. When crystallization waves are mechanically excited, the surface of a 4 He crystal goes into a dynamic state of quantum roughness, similar to a thermodynamic equilibrium state of atomic roughness found at the surface of a classical crystal (see Phase transitions at a surface). The spectrum of crystallization waves at low frequencies has the form: ρL k 3 ρL k +g ρS − ρL (ρS − ρL )2 ρL ρS − iωk , K(ρS − ρL )

ω2 = α

where ω and k are the frequency and the wave number of the crystallization waves; ρ L and ρ S are the densities of the liquid and the solid, respectively; g is the free fall acceleration (9.8 m/s2 ); K is the kinetic coefﬁcient of growth (proportionality coefﬁcient between rate of growth of a rough crystal face, and difference between crystal and liquid chemical potentials); α = α + ∂ 2 α/∂ϕ 2 is the surface rigidity of a given face of the crystal (α is the speciﬁc surface energy, and ϕ is the crystallographic angle corresponding to the direction k). The value of K for helium is particularly large below 0.7 K so propagating crystallization waves are only weakly damped. CRYSTALLOGRAPHIC CLASSES The same as Crystal classes. CRYSTALLOGRAPHIC INDICES

A triplet (quadruplet) of numbers deﬁning the position of points (sites), directions and planes in a lattice. Let the radius-vector from the origin to a given site in the crystal lattice be projected on to the a, b, c axes in a (in general, oblique) coordinate system so that these projections are equal to ax, by, cz. Then x, y, z are the crystallographic indices of that site, and the direction of

250

CRYSTALLOGRAPHIC SYSTEM Table 1. Crystallographic classiﬁcation scheme System

Triclinic (anorthic) Monoclinic Orthorhombic Trigonal Hexagonal Tetragonal Cubic (isometric)

Number of

Example of point group

space groups

International

Schönﬂies

2 13 59 25 27 68 36

1 2/m mmm 3m 6/mmm 4/mmm m3m

Ci C2h D2h D3d D6h D4h Oh

a vector to that site is denoted by [xyz]. A vector parallel to the x coordinate axis is in the [100] direction, etc. Crystallographic planes are denoted by what are called Miller indices (hkl). Consider a plane which intersects the a, b, c axes at the points h a, k b, l c, and write down the reciprocals of these intercepts 1/ h , 1/k , 1/ l . The Miller indices are the smallest three integers h, k, l having these same ratios. For example, if h = 4, k = 1 and l = 2 then (hkl) = (142). The three integers which deﬁne orientation directions in a crystal, and the positions of its verges, are called the Weiss indices, and they are written in the form [p1 p2 p3 ]. As for the hexagonal system and the trigonal system, their directions and planes are sometimes presented in a four axes system (three equivalent directions are then positioned at 120◦ to each other in the basal plane of the crystal). The Bravais indices [mnrp] and (hkil) satisfy the conditions r = −(m + n), i = −(h + k). When using the Bravais indices one may clearly see the equivalence of the respective directions and planes in the crystal. CRYSTALLOGRAPHIC SYSTEM

Crystallographic classiﬁcation scheme for the 230 space groups that takes into account their characteristic symmetries (see Crystal symmetry), and uses the ratios of their symmetry axes. There exist seven independent combinations of the rotation symmetry axes of the nth order (n = 1, 2, 3, 4, 6), and seven crystallographic systems corresponding to them: cubic system, hexagonal system, trigonal system, tetragonal system, orthorhombic system, monoclinic system and triclinic system. The concept of crystallographic system

coincides with the concept of syngony for every crystallographic system, with the exception of the hexagonal and the trigonal systems which together comprise the hexagonal syngony or family. Table 1 outlines the crystallographic classiﬁcation scheme, and lists a high-symmetry point group for each system. CRYSTALLOGRAPHIC TEXTURE See Texture. CRYSTALLOGRAPHY (fr. crystal, and Gr. γραϕω, am writing) The science describing crystals and the crys-

talline state of matter. Six basic branches are recognized within crystallography: geometric crystallography (crystal symmetry, crystal structures, and crystal morphology); crystallogenesis (crystal formation and growth, see Crystallization); crystal physics; crystal chemistry; applied crystallography (methods and techniques for crystal growth and use in technical applications); space crystallography or growing crystals in zero gravity (in orbit) and studying their properties. Geometric crystallography gave birth to the hypothesis of ordered three dimensional positioning of particles (atoms and molecules) composing the crystal which form the crystal lattice. The mathematical apparatus of crystallography is based on Euclidean geometry, group theory, and tensor calculus. Structural crystallography studies the atomic and molecular composition of crystals using X-ray structure analysis, electron diffraction analysis, and neutron diffractometry, all based on the diffraction of waves and particles within the crystals. Optical spectroscopy, electron microscopy, and

CRYSTAL MORPHOLOGY

resonance methods, etc., are sometimes used. As a result, the crystal structures of over a hundred thousand chemical substances have been determined. When studying the processes of formation and growth of crystals one uses the basic principles of thermodynamics, the laws of r st-order phase transitions, and of surface phenomena. One also accounts for the interaction of crystals with their ambient environment, and for anisotropies. Industrial processes used to grow diamonds, rubies, and other crystals have been perfected (see Synthetic monocrystals), and provide a basis for quantum and semiconductor electronics, optics, acoustics, etc. Crystallography also studies various perturbations in an ideal crystal lattice, such as defects and dislocations, that originate during the course of crystal growth due to various external inﬂuences, and inﬂuence many properties of crystals. The structure and properties of various aggregates formed from microcrystals (polycrystals, textures, ceramics), as well as substances with atomic ordering similar to that found in crystals (liquid crystals, polymers), are also studied. Consistent symmetrical and structural patterns studied within the framework of crystallography ﬁnd their application when treating general structural features and properties of various non-crystalline states of condensed matter, such as amorphous solids and liquids, polymers, macromolecules, supermolecular structures, etc. (generalized crystallography). Studies of biological crystals have been successful in determining the structures of large protein and nucleic acid molecules. Modern crystallography typically concentrates on the atomic and defect structure of crystals, processes of their formation and growth, and searches for new properties of crystals. These problems involve comprehensive tasks aiming at discovering new materials with important physical properties. Results obtained from crystallographic studies are routinely applied to physics, mineralogy, chemistry, molecular biology, etc.

CRYSTAL MORPHOLOGY (fr. Gr. μoρϕη , appearance, shape, and λoγ oς , word) Outward shape of crystal that grows from a

solid, liquid or gaseous phase. It depends on the nature of the substance, on growth conditions, and other factors. During crystallization from the melt with a small deviation from equilibrium, crystals of some materials grow in the shape of regular crystal polyhedra (Fig. 1), while crystals of other materials grow in a shape approximating a sphere (Fig. 2(a)). A faceted shape (see Crystal faceting) is typical of materials that exhibit a high entropy of fusion S = L/T > 4R (L is the latent heat of melting, R is the gas constant), and a high anisotropy of surface energy. A rounded shape is typical of metals and other materials that exhibit a low entropy of fusion ( S < 4R) and a low surface energy anisotropy. Metals grown from a gaseous phase or from solution may exhibit a faceted shape. A smooth shape loses stability and develops bulges (Fig. 2(b)) at increased overcooling of the melt (in metals, this process occurs at smaller values of overcooling, than in crystals with a high entropy of fusion). The presence of impurities intensiﬁes this process owing to emerging structural overcooling. Thermal and structural overcooling ﬁrst results in the formation of bulges (cellular morphology), which then evolve into dendrites (Fig. 2(c, d)). Under sufﬁciently high overcooling, the dendritic shape degenerates into a needle one without lateral branches. When crystallization takes place from a viscous medium,

CRYSTALLOGRAPHY, INTERNATIONAL TABLES See International Tables for Crystallography. CRYSTALLOGRAPHY, TWO-DIMENSIONAL See Two-dimensional crystallography.

251

Fig. 1. Crystal polyhedron.

252

CRYSTAL NUCLEI

Fig. 2. Crystal morphologies.

spherulites form, which are monocrystalline ﬁlaments or crystallite aggregates of radial-beam shape. CRYSTAL NUCLEI, crystallization centers

Crystal phase clusters of critical (and larger) sizes with the capability of growing (see Crystallization) in a melt. The critical size of a crystal nucleus is associated with the equality of the bulk and the surface parts of its free energy (which decreases as the melt is overcooled). Crystallization centers may appear spontaneously on solid surfaces, where this process is facilitated by the formation of crystal nuclei.

CRYSTAL OPTICS

The branch of optics investigating light propagation in crystals. Among phenomena of crystal optics, there are birefringence, interference and polarization of light, optical activity (see Rotation of light polarization plane), conical refraction of light, pleochroism, etc. These phenomena can appear or vary under the action of external electric and magnetic ﬁelds, mechanical stress, acoustic waves, and this is the subject of electron, magnetic, piezo-, and acoustic optics, respectively. The classical approach to the phenomena of crystal optics is based on the electrodynamics of continuous media, crystal symmetry, tensor cal-

CRYSTAL OPTICS

culus; it is based on the fact that the period of a crystal lattice (∼1 nm) is much shorter than the wavelength of light (∼500 nm), and therefore, a crystal can be considered as a homogeneous anisotropic medium. This is expressed by a tensor form of material equations connecting the electric ux density Di and magnetic ux density Bi with the corresponding ﬁelds Ej and Hj : Di = εij Ej and Bi = μij Hj (here εij and μij denote the polar tensors of rank two of dielectric constant and magnetic permeability). In most problems of crystal optics, one considers nonmagnetic crystals (μij = 1) and concentrates upon the properties of the tensor εij . In the absence of spatial dielectric dispersion, the dissipation of energy, and an external magnetic ﬁeld, by the symmetry principles of kinetic coefﬁcients, the tensor εij is symmetric and real. Therefore, for a ﬁxed frequency of light ω, in anisotropic media, the directions of vectors D and E do not coincide. This determines the anisotropy of the optical properties of crystals, i.e. the dependence of the phase veloc√ ity v = c/n and of refractive index n = ε on the direction. For the totality of all directions at an arbitrary point of a crystal, the magnitudes of n form an ellipsoidal surface, which is called the optical indicatrix. The symmetry axes of the optical indicatrix form three mutually orthogonal principal directions in the crystal (crystallophysical axes), along which the directions of vectors D and E coincide. In the rectangular Cartesian coordinate system with axes coinciding with the crystallophysical axes, the equation of the optical indicatrix is of the form x2 n2x

y2 z2 + 2 + 2 = 1, ny nz

where nx , ny , and nz are the principal values of n. Crystals of a cubic system are optically isotropic, i.e. their ellipsoid degenerates into a sphere; the crystals of medium systems are optically uniaxial (the indicatrix is an ellipsoid of revolution); the crystals of lower systems are optically biaxial (the indicatrix is a triaxial ellipsoid). The optical axis of a crystal corresponds to the normal of a circular section of the optical indicatrix. The laws of propagation of plane harmonic waves in dielectric crystals follow from the wave

253

equation together with the tensorial relation between the vectors D and E. Thus, we get the dispersion equation, which corresponds to a homogeneous system of three linear equations for the components of the vector E: εij (ω)ω2 2 δ + k k E (ω) = 0, − k ij i j j c2 where k, ki , and kj are the magnitudes of the wave vector and its corresponding components, δij = 0 for i = j , and δij = 1 for i = j . This system has a nontrivial solution E = 0 if and only if the determinant in the parentheses is not zero. The latter condition leads to the Fresnel equation ky2 kz2 + + = 0, v 2 − vx2 v 2 − vy2 v 2 − vz2 kx2

where v is the magnitude of the phase velocity, the direction of which coincides with the direction of the wave vector k; vx , vy , and vz are the principal phase velocities of the wave for the corresponding directions of the vector D when the light propagates along one of the principal directions. The dispersion and Fresnel equations are quadratic with respect to k and v, i.e. at light propagation in anisotropic crystals, there arise two waves (see Fig.) with different values of the magnitude of the wave vector and different phase velocities (refractive indices) v1 and v2 coincide only along the directions of the optical axes. They correspond to two mutually orthogonal values of the vectors D and E. If from some point of the crystal one locates all the vectors corresponding to v1 and v2 in all the directions m, then the endpoints of these vectors form two surfaces called the surfaces of normals. In uniaxial crystals, one of these surfaces is a sphere (characterizing the ordinary ray v0 ), and the other one is an ellipsoid of revolution (characterizing the extraordinary ray ve ) tangent to the sphere at its intersection points with the optical axis. In biaxial crystals, both surfaces are ellipsoids intersecting at 4 points lying pairwise on two optical axes (binormals). The ray vectors form similar surfaces called ray surfaces (or wave surfaces). Thus, in anisotropic crystals, in an arbitrary direction m, there may propagate two plane waves polarized in two mutually orthogonal planes. The

254

CRYSTAL, PERFECT

Crystal optics.

directions of vectors D 1 and D 2 of these waves coincide with axes of the ellipse of the central section of the optical indicatrix by the plane orthogonal to m, and the lengths of the ellipse axes determine their refractive indices. Consequently, the optical indicatrix and surfaces of normals are mutually dependent. The birefringence in the crystals because of the different refraction indices of two polarized waves propagating in the same direction implies a path difference. If, in a convergent light, one reduces the polarization of these waves into one plane (using some polarization devices), this results in the interference of the light. Such interfering conoscopic images allow one to investigate crystal-optical properties of crystals. In the presence of a spatial dispersion of ﬁrst order with respect to k or an external magnetic ﬁeld, and also in magnetic crystals, the tensor εij is complex and, in general, nonsymmetric; moreover, εij (ω, k, H ) = εij (ω, −k, −H ). In particular, in such crystals two elliptically polarized waves propagate with orthogonal axes of the ellipse coinciding with the axes of the section ellipse of the optical indicatrix. The directions of by-pass of vectors E are opposite in both waves. Along the direction of the optical axis, and in cubic crystals, the polarization ellipses degenerate into circles, i.e. the waves are circularly polarized and have

different velocities. Moreover, in uniaxial crystals, the surfaces of normals do not osculate at the points of intersection with the optical axis. The ellipticity of waves brings about optical activity of crystals, which is expressed, e.g., as gyration, electrogyration, Faraday effect, etc. The complexity of the tensor εij and the elliptical two-ray refraction are also caused by light absorption in crystals. The directions of by-pass of ellipses in this case coincide. In such crystals, the absorption of differently polarized waves is different, and occasionally circular dichroism takes place in optically active crystals. Crystal optics adjoins crystallography, solid state physics, and mineralogy. With the appearance of laser technology, new branches of physical optics and optical tool making arose that are fundamentally based on crystal optics: coherent and nonlinear optics, holography, optoelectronics, integrated optics, etc. The control of optical (in particular, laser) radiation is based on the phenomena of crystal optics. CRYSTAL, PERFECT See Perfect crystal, Ideal crystal. CRYSTAL PHYSICS, physical crystallography Branch of crystallography involving the physical properties of crystals and crystalline aggregates of polycrystals, as well as changes in their

CRYSTAL PHYSICS

properties arising from external inﬂuences. Crystal physics explains anisotropy of crystals, and basic variations in the properties of crystals due to the regular distribution of particles (molecules, atoms, and ions) in the crystal lattice, and the types of their interrelations. The mathematical apparatus of matrix algebra, tensor calculus, and group theory provides a quantitative description of the physical properties of crystals. Directionally independent properties such as density are characterized by scalar variables. To describe physical properties involving relationships between two vectors (e.g., between either polarization or electric current density and electric ﬁelds, etc.) or between pseudo-vectors (e.g., magnetic induction and magnetic ﬁeld strength) one uses second-rank tensors (e.g., dielectric constant and magnetic permeability tensors). Many physical ﬁelds in crystals (e.g., electric and magnetic ﬁelds, mechanical strains) are themselves tensor ﬁelds. The relation between the physical ﬁelds and the properties of crystals may be described by tensors of higher rank, as is the case with the piezoelectric effect (see Piezoelectricity), electrostriction, magnetostriction, elasticity, photoelastic tensor, etc. It is convenient to represent dielectric, magnetic, elastic, and other physical properties of crystals in the form of characteristic surfaces such as ellipsoids. The radius-vector that traces out such a surface indicates the value of a particular property along its given direction (see Crystallographic indices). The symmetry of any property of a crystal may not be lower than the symmetry of its external shape (Neumann principle, F. Neumann). In other words, a symmetry group G1 that describes any physical property of a crystal includes necessarily the symmetry elements of its associated point group G, that serves as its supergroup: G1 ⊃ G. The symmetry elements determine the orientations of the principal axes of characteristic surfaces, as well as the number of tensor components that determine a given physical property. In many cases these are surfaces of ellipsoids with their principal axes related to the symmetry axes of the crystal (see Crystal classes). Crystals of low symmetry have their physical properties described by second-rank tensors with three principal values (plus the orientation of the tensor principal axes). Physical properties of cubic symmetry crystals that are described by second-rank tensors are

255

directionally independent or isotropic. Crystals of intermediate symmetry (tetragonal, trigonal and hexagonal) have these properties characterized by the symmetry of their rotation ellipsoid, i.e. their second-rank tensors have two independent components, one of which describes the property along the principal axis, and the other along any direction orthogonal to this axis. To describe the property along an arbitrary direction one needs to know these two principal components plus the direction cosines of the direction. Physical properties described by higher-rank tensors are characterized by a larger number of parameters: e.g., elasticity properties, described by a fourth-rank tensor, need three such variables in a cubic crystal, and two independent variables in an isotropic medium. The elastic properties of a triclinic crystal require 21 independent tensor components for their description. To determine the number of independent components of tensors of higher rank (5th, 6th, etc.) one can make use of the corresponding point group of symmetry. To obtain a complete description of the physical properties of crystals and textures one may make use of radiofrequency, acoustical, optical, and other techniques. Crystal physics studies both phenomena speciﬁc for anisotropic media (birefringence, rotation of light polarization plane, direct and inverse piezoeffects, electro-optic, magneto-optic, and piezooptic effects, generation of optical harmonics, etc.), as well as properties more often associated with isotropic media (electric conductivity, elasticity, etc.). In crystals these latter properties may also exhibit features resulting from the crystal anisotropy. Many phenomena within the scope of crystal physics are related to changes in the crystal symmetry under various thermodynamic conditions. The Curie principle may be used to predict changes in both the point and the space symmetry groups of crystals undergoing phase transitions, e.g., entering ferromagnetic or ferroelectric states (see Ferromagnetism, Ferroelectricity). Crystal physics studies various defects of the crystal lattice (color centers, vacancies, dislocations, grain boundaries, stacking faults, domains, etc.) and their effects upon the physical properties of crystals (plasticity, strength, luminescence,

256

CRYSTAL POLYHEDRON

electrical conductivity, mechanical Q-factor, etc.). Among the tasks of crystal physics is the search for new crystalline materials with speciﬁc prospective properties needed for practical technological applications. CRYSTAL POLYHEDRON A monocrystal grain under equilibrium conditions (see Monocrystal growth) consisting of a

certain combination of faces, edges and vertices. The number of faces, edges and vertices should follow the Euler theorem (L. Euler): the sum of the number of faces and vertices equals the number of edges plus two (F + V = E + 2). The socalled simple forms participate in crystal faceting. These are polyhedra whose faces can be obtained from one another via symmetry operations that are speciﬁc for the crystal class of the given crystal; they usually form various combinations with each other. There are 47 geometrically distinct simple forms known; this number increases to 193 when taking into account enantiomorphous (mirror reﬂection) pairs (see Enantiomorphism), or to 146 in case one accounts for differences in point symmetry. Only certain simple forms are permissible in each point group. Speciﬁc forms of crystal polyhedra depend on their structure and conditions of crystallization. CRYSTAL, QUANTUM See Quantum crystals. CRYSTALS (fr. Gr. κρυσ τ αλλoς , ice) Solids with ordered three-dimensional periodic

spatial atomic structure. The formation medium may be an overcooled vapor or liquid of a pure substance, a supersaturated solution or ﬂux of one material in another (the solvent), or a crystal medium of a polymorphous modiﬁcation or composition different from that of the newly formed crystal. Some features of crystals depend on their formation process. If the material is supplied evenly and uniformly from the ambient environment then a polyhedral shape results, limited by ﬂat faces intersecting each other along straight edges. These faces, often mirror smooth in perfect crystals, are tilted toward each other at certain angles characteristic for the particular crystal type (law of constancy of angles). The ratios between

the intercepts on the axes for different tilted faces of a crystal can always be expressed by rational numbers such as 1 : 2 √ or 2 : 3, and never by irrational ones such as 1 : 2 (law of rational indices). Other general macroscopic properties of crystalline matter include crystal homogeneity (independence of the choice of measurement point), anisotropy of crystals (dependence on direction), and crystal symmetry (spatial transformations that bring the crystal into itself). There are 32 classes of morphological symmetry of crystals, each corresponding to its speciﬁc set of symmetry elements: axes, planes, center of symmetry, etc. Three-dimensional atomic structure periodicities are described in terms of a threedimensional space lattice (the crystal lattice), a three-dimensional periodic system of points that may be formed starting from an arbitrary point by simply repeating the lattice by a series of parallel translations. There exist a total of 14 types of such lattices called Bravais lattices. The crystal appearance (crystal morphology) is characterized by the crystal shape and faceting, i.e. the set of faces bounding the crystal, and by the ratio of the sizes of these faces (see crystal faceting). Such facets and their relative sizes characterize the crystal morphology or crystal habit. The shapes of crystals reﬂect their crystal structure, and the nature of the interactions between their atoms. In particular, these factors affect the shape of the forming crystal through kinetic phenomena occurring at the surface of a growing crystal. Such phenomena depend on the level of supersaturation, temperature, composition of the ambient medium, thermal conductivity, diffusion, and the presence of impurities. The shape acquired by the crystal during its growth (the growth shape) is very sensitive to the conditions of crystallization, and reﬂects the mechanism of growth. Therefore, the growth shape implies certain conclusions beyond the conditions of growth. During the artiﬁcial growth of crystals the crystallization parameters may be chosen accordingly. Although a typical crystal shape is a polyhedron, rounded growth shapes or strongly perturbed shapes may form under certain ambient conditions (thread-like crystals, plates, dendrites, etc.). Some crystals can form in two different modiﬁcations, a right-hand and left-hand one (enantiomorphism). Substances

CRYSTAL STABILITY CONDITIONS

are found that may crystallize in the shape of twins (twinning of crystals). In cases when crystal faceting is suppressed by the limited availability of feeding material, forced growth shapes develop. The crystal can then acquire the shape of the surface limiting its growth (e.g., crucible walls, smelting isotherm in a smelt, an isoconcentration saturation surface in a gas phase). Most monocrystals are the result of forced growth. Technologies for growing crystals with forced growth shapes ﬁnd wider and wider applications. Almost all semiconductor crystals are produced that way, as well as most piezoelectric, ferroelectric, and optical crystals (see Monocrystal growth). If crystal generation and growth occur simultaneously throughout the whole volume a polycrystal forms, that is an aggregate of randomly oriented ﬁne crystals of various sizes and shapes called crystallites or crystal grains. Sometimes crystallites follow a certain predominant orientation indicating the presence of a texture. During mass crystallization when embryos appear only in certain regions of the generating medium, the collective growth of crystals ensues, characterized by the interaction of the growing crystals with each other, to produce a geometric selection. Crystals having an optimal orientation for the given ambient conditions then survive. Such a competition results in the formation of a pole structure, typical for metal ingots, in which all the crystals are elongated and almost parallel to each other. Examples of such collective growth are druses (crystal agglomerations in which the vertices of separate crystals face in more or less the same direction) and parallel inshoots (crystals growing together to merge in a parallel orientation). The ideal structure of a crystal always undergoes certain perturbations (accumulates defects) because growth conditions change, impurities are trapped, and various external inﬂuences are always at work. Real crystals often display macrodefects (gas–liquid, solid inclusions, cracks, etc.) which worsen their properties. A typical structural defect is mosaicity (see Mosaic crystals) which results from various defects (internal stress, block boundaries, twins (see Twinning of crystals), stacking faults, dislocations, etc.) that appear during crystal growth. The presence of foreign atoms and ions (impurities) in a crystal during its growth may result in the development of zonal, sectional, and

257

other structures. Substituting crystal atoms (substitutional impurities) or imploding between the atoms of the crystal (implosion impurities) can produce point defects (see Impurity atoms). Other point defects perturbing the lattice periodicity are vacancies and interstitial atoms. The level of deﬁciency of the crystal structure affects both crystal growth (e.g., the dislocation mechanism of growth) and various crystal properties that are structure sensitive (plasticity, strength, electrical conductivity, photoconductivity, light absorption capacity, etc.). Therefore, to grow crystals with prescribed properties, one must intentionally introduce desired defect structures. Examples are donor and acceptor impurities which determine the electrical properties of semiconductors. Added impurities (doping) are widely used to produce semiconducting crystals with various types and levels of conductivity, to produce laser crystals with a prescribed spectral transmission band, etc. The development of electronics, quantum electronics, computer technology, and various other industries is directly linked to using crystals and complex crystal structures based on them (e.g., epitaxial layers, heterostructures, microchips, superlattices). CRYSTAL STABILITY CONDITIONS

Conditions imposed on the coefﬁcients of the expansion of the crystal potential energy U in terms of atomic displacements usi : U = U0 + Asi usi s,i

+

1 Ast ij usi utj + · · · , 2 s,t,i,j

where U0 is the crystal energy at equilibrium (the indices s and t are used for labeling atoms; i, j = x, y, z). From the condition that the resultant of all forces acting on the atoms at equilibrium vanishes, it follows that Asl = 0. From the inrotation of variance of U under translation and the crystal as a whole it follows that t Ast ij = 0, t (Ast ij Xt k − Ast ik Xtj ) = 0 (Xsi designates the sth atom coordinates). Crystal symmetry properties impose additional restrictions on the harmonic force constants Ast ij , and the application of these relationships considerably reduces

258

CRYSTAL STRUCTURE

the number of independent force constants. Besides that, some restrictions on the force constants follow from the condition of crystal equilibrium (U = min at equilibrium), and these are in the form of inequalities arising from the requirement of positive deﬁniteness for the quadratic form (third term) of the expansion of U . Similar conditions may be derived for the anharmonic force constants, which serve as the coefﬁcients of additional terms of the expansion of U . CRYSTAL STRUCTURE

The structure of an actual crystalline solid. The concept of crystal structure starts with the concept of crystal lattice, i.e. of the parameters of a unit cell, such that any ideal crystal (monocrystal) may be reproduced by repeating its unit cell in space. A full description of a crystal structure also includes specifying the positions of atoms, ions and molecules inside the cell (including the orientations of molecules). Beside the locations of the atoms, other important factors are the distribution of the electron density in the unit cell, the atomic and ionic radii, chemical bonds (see Crystal chemistry), coordination numbers (see Coordination sphere), etc. Ferroelectric and magnetic crystals are also characterized by the direction of their electric and magnetic moments, respectively. The corresponding lattices may not necessarily coincide with the crystallographic ones, and they may possibly be mutually incommensurate. The crystal structure of an actual crystal is quite variable, thus opening ways for numerous practical applications. Speciﬁc branches of the physics of solids are dedicated to their description (see Crystal physics). The concept of crystal structure also includes various lattice defects: point defects (such as vacancies, interstitional or substitutional impurity atoms, atomic clusters); linear defects (dislocations); two-dimensional defects (stacking faults, twins, etc.). When studying the crystal structure of solid solutions one has to know the distribution of atoms (ions, molecules) of various types in their sublattices. Crystal structure also includes describing the physical composition and parameters of structural elements (grains, cells, and blocks) and various other factors.

The main techniques for studying crystal structures are X-ray diffraction structural analysis, neutron diffraction, and electron diffraction. CRYSTAL SYMMETRY, microscopic crystal symmetry

Geometrical regularity in the spatial arrangement of particles (atoms, ions, molecules, complexes), composing a crystal. One can characterize the symmetry of a crystal by the totality of all spatial transformations (x , y , z ) = f (x, y, z), which bring the crystal into coincidence with itself. From all conceivable transformations it is sufﬁcient to restrict attention to linear ones, and not necessarily to all of these, but only to deformationfree types, i.e. to linear orthogonal transformations that preserve the lengths of segments and angles between them: (x , y , z ) = α(x, y, z) + (x0 , y0 , z0 ), where α is the transformation matrix. The determinant D = |α| in this case can have only two values D = ±1. The transformations with D = 1 are called proper transformations, and all of them involve rotational spatial displacements (i.e. rotations) around some axis through an angle ϕ, while transformations with D = −1 are called improper; the unit improper transformation being inversion (x , y , z ) = (−x, −y, −z). All improper transformations are combinations of proper transformations with inversion. In general a linear transformation can involve a shift or translation, designated by the term (x0 , y0 , z0 ) through a distance appropriate to the crystal structure lattice spacings. If the term (x0 , y0 , z0 ) = 0 there is no translation, and the transformation is either a proper rotation for D = +1, or an improper rotation for D = −1. The three-dimensional periodicity of a crystal automatically sharply restricts the possible angles ϕ of allowed proper (and improper) rotations to ﬁve values: 0◦ , 60◦ , 90◦ , 120◦ and 180◦ . It is customary to express the allowed angles ϕ by the expression ϕ = 2π/n, and in the international notation to designate proper rotations by the ﬁve integers: n = 1, 2, 3, 4, 6. Improper rotations are ¯ 2¯ = m, 3, ¯ 4, ¯ 6, ¯ where m is the designated by 1, symbol for a mirror reﬂection in a plane. In the older Schönﬂies notation the proper and improper rotations are designated, respectively, by C1 , C2 , C3 , C4 , C6 , I , S2 = σ , S3 , S4 , S6 . There are

CRYSTAL SYSTEM

two special combined rotation-translation symmetry operations: (a) a screw rotation which is a rotation by 2π/n combined with a translation by half a lattice spacing along the rotation axis, and (b) a glide reﬂection which is a reﬂection in a plane combined with a translation by half a lattice spacing parallel to the plane. The complete set of all available symmetry transformations of a crystal form the space group of the crystal (called Fedorov group in the Russian literature). It is discrete, but with an inﬁnite set of elements, because translation through all possible periods is endless. There exist 230 possible space groups, and they are described explicitly in the International Tables for Crystallography. Also important in the physics of crystals are ﬁnite groups containing only proper (and possibly improper) rotational elements (without translations) which are called crystal classes or point groups, and their number is only 32. In three dimensional space there are only 14 translational groups which contain no rotational elements. A set of points invariant under translation form a crystal lattice (Bravais lattice). Each space group has associated with it a point group and a crystal lattice. When describing the symmetry of magnetic (magnetically ordered) crystals (see Magnetism), the situation becomes complicated, since transforming a crystal into itself requires matching not only coordinates of individual identical atoms, but also the directions of their atomic magnetic moments (spins). The Shubnikov extension of symmetry theory to the symmetry of magnetic crystals involves the addition of the non-spatial operation R of spin reversal (see Shubnikov groups). The addition of this new symmetry element permits one to construct 1651 space (Shubnikov)

259

groups, 122 point groups and 36 translational magnetic symmetry groups (see also Antisymmetry). A further generalization brought about the appearance of the theory of colored symmetry, and the creation of many additional colored symmetry groups. All these types of groups ﬁnd use in solid state physics. Concerning macroscopic physical properties (optical, electrical, mechanical, magnetic, etc.), crystals behave as media that are homogeneous, but anisotropic (see Anisotropy of crystals); and the discreteness of their atomic structure is not signiﬁcant. Because of this only the rotational symmetry of a crystal, i.e. its point group, is of importance for the macroscopic directionally dependent properties described by tensors of different ranks. Then the distinction between crystals by their differences in symmetry ﬁnds its expression in the intrinsic symmetry of tensors for different physical properties. The literature provides information on the speciﬁc forms of various tensors of many ranks for all 32 of the crystallographic point groups.

CRYSTAL SYSTEM

The classiﬁcation of crystals in accordance with their crystallographic coordinate system, i.e. by the metric represented by the set of independent linear (a, b, c) and angular (α, β, γ ) crystal lattice constants. It is possible to choose seven different unit cells with the same number of crystal systems corresponding to them (see Table 1). The concept of syngony (in common use in the Russian literature) coincides with the concept of crystal system for all crystal systems except the hexagonal.

Table 1. Unit cell shapes and metric parameters for the seven crystal systems Crystal system

Shape of unit cell

Metric parameters

Triclinic Monoclinic Orthorhombic Tetragonal Hexagonal Trigonal Cubic

Oblique-angled parallelepiped Straight prism with parallelogram in base Right-angle parallelepiped Right-angle parallelepiped with square in base Prism with base in rhombic shape, γ = 120◦ Rhombohedron Cube

a, b, c, α, β, γ a, b, c, β a, b, c a, c a, c a, α a

260

CRYSTAL, THREAD-LIKE

CRYSTAL, THREAD-LIKE See Thread-like crystals. CUBIC SYSTEM A crystallographic system deﬁned by the presence of four third-order symmetry axes (C3 ) in crystals with cubic symmetry. The unit cell of the

system is a cube with lattice parameter a. The coordinate axes of a cubic system contain 4, 4, and 2 (i.e. C4 , S4 , and C2 ) symmetry elements. This system includes three Bravais lattices (primitive, body-centered, face-centered), ﬁve point groups (T , Th , Td , O, Oh ), and 36 space groups (see Crystal symmetry). CUMULATIVE EFFECT

Accumulation is a process of building up the energy ﬂux density in a medium by focusing the ﬂows of energy. It is achieved either through speciﬁc shaping of an elongated energy source, or through the interaction of shock waves. This effect is usually produced using explosives. In solids this may be realized in several ways, as follows. Cumulative jets are formed by compressing metal linings placed into the cumulative cavities in explosive charges. The shape of the lining may be hemispherical, conical, parabolic, hyperbolic, etc. Compression concentrates the principal part of the explosive energy into a thin internal layer of the lining so that this layer forms a cumulative jet. The mass of metal transformed into the jet may reach 6–20% of the total mass of the lining, and the energy density in the jet may reach 106 MJ/m3 . Shock wave collision. During a frontal collision of shock waves in a solid (see Explosion) each element of the solid is sequentially compressed ﬁrst by the incident and then by the reﬂected shock wave. As a result, pressures in the area of the reﬂected shock wave exceed those in the incident wave by a factor of several times, while temperatures remain comparatively low, that is lower than those resulting from compression by a single shock wave. During a glancing collision of shock waves that meet at a certain angle a triple shock wave conﬁguration forms, and pressures in its forward wave signiﬁcantly exceed those produced during a frontal collision. By means of this technique a pressure of 1.8 TPa was achieved in copper samples.

Cumulation in a medium with varying density. When a shock wave exceeding a critical value passes through a system of gradually tapering alternating layers of light and heavy material its propagation develops into a periodic selfreinforcing process (see Self-similarity) that results in the unlimited growth of pressure at its front. CUNICO

Hard magnetic material based on the Cu–Ni– Co system. A high-coercive state is achieved upon quenching from 1100 ◦ C and tempering at 625 ◦ C. Cunico alloys are readily plastically deformable, so they are employed for the manufacture of permanent magnets of a complicated shape. For properties, see Table 1 in Hard magnetic materials. CUNIFE

Hard magnetic material based on the Cu–Ni– Fe system. A high-coercive state is achieved upon quenching from 1100 ◦ C, tempering at 700 ◦ C, applying cold strain with high compression, and tempering at 650 ◦ C. The strain induces uniaxial magnetic anisotropy along the rolling or drawing direction. Cunife alloys are used as thin wires or stampings. For properties, see Table 1 in Hard magnetic materials. CURIE GROUP

See Limiting symmetry groups. CURIE LAW (1895)

Temperature dependence of the magnetic susceptibility, χ = C/T , in many paramagnets, where C is the Curie constant (C > 0). All gases in which the atoms, molecules, or ions have permanent magnetic moments follow the Curie law, as well as dilute liquid solutions of transition metal ions, as well as crystals of compounds of these elements with non-metallic bonding. It holds for temperatures at which the thermal energy signiﬁcantly exceeds the energy of interaction of neighboring ionic magnetic moments with each other, and with the external magnetic ﬁeld.

CURIUM

For subsystem properties, the case

CURIE POINT, Curie temperature

The point (temperature TC ) of a second-order phase transition. Examples of a Curie point are the temperatures TC of magnetic phase transitions, ferroelectric phase transitions, structural phase transitions, and other phase transitions in solids. Special names are used for certain transitions, such as the Néel point for the antiferromagnetic Curie point. CURIE PRINCIPLE (P. Curie, 1984)

This principle deals with the symmetric aspect of the causality principle. Namely, the symmetry of a system of causes is (abstractly) preserved in the symmetry of the outcomes. This principle is a philosophical generalization of the Neumann– Minnegerode–Curie principle which states that the symmetry of physical properties of a system made of a material object (e.g., a crystal) and of an external action is not lower than the intersection (a general subgroup) of the groups of symmetry of the object and action. The Curie principle holds for all deterministic systems, to which the notion of symmetry can be applied. A modern formulation of the Curie principle establishes a homomorphism relation in the particular case of an isomorphism between the symmetry groups of a system of causes Gcsys and a system of outcomes Gout sys : Gout sys =

!

sym

Gout j Gout

↔

!

sym

Gcj Gc

= Gcsys .

For a homogeneous system, parts of which are connected by some symmetrizer Gsym , its symmetry is deﬁned by the intersection of the sym" metry groups of its parts, Gj = G1 ∩ G2 ∩ · · ·, multiplied by Gsym (the Shubnikov theorem). For an inhomogeneous system, Gsym reduces to identity and the " system symmetry is deﬁned by the intersection Gj (the Curie theorem). Taking, e.g., the interaction of an object with an external action as the cause of a physical phenomenon, we ph can ﬁnd the symmetry group Gj of a systemsym

atic phenomenon (for Gc case,

= 1), or in a particular

Gobject ∩ Gaction = Gcsys .

261

ph

c Gout j ↔ Gj ← Gsys sym

is possible if Gc = 1 (the Wigner theorem). This systematic formulation explains violations of the Curie principle associated with the incompleteness of a given system of causes, an inexact deﬁnition of symmetry of the system components, or with using the Curie theorem instead of the Shubnikov theorem. CURIE–WEISS LAW (P. Curie, P. Weiss, 1907) The temperature dependence of the susceptibility χ of ordered systems above the point of their transition to an ordered phase at the Curie point TC

has the form: χ = χ0 +

C , T −θ

where C is the Curie constant, χ0 is the temperature independent part of the susceptibility, and θ is the characteristic temperature. For the magnetic susceptibility χ of paramagnets, or ferromagnets in their paramagnetic phase above TC , as well as for the dielectric susceptibility of ferroelectrics and other materials, θ is called the Weiss temperature, or sometimes the Curie–Weiss temperature. The value of θ depends on particle interactions, and may differ appreciably from TC (see also Dielectric constant). In the case of antiferromagnets (or antiferroelectrics) and virtual ferroelectrics the value of θ may become negative. The Curie–Weiss law holds for the range of temperatures in which the ﬂuctuations are not critical uctuations, that is for (T − TC )/TC Gi, where Gi is the Ginzburg number. CURIUM, Cm

A chemical element of Group III of the periodic system with atomic number 96 and atomic mass 247.07; it is a member of the actinide family. 15 isotopes are known with mass numbers 238 to 252, none of them being stable. The electronic conﬁguration of the outer shells is 5f 7 6d 1 7s 2 . The ionization energy is 6.09 eV. Atomic radius is 0.1749 nm; radii of Cm3+ and Cm4+ ions are 0.0946 and 0.0886 nm, respectively. Oxidation state is +3 (more rarely, +4, +6).

262

CURRENT CARRIER DRIFT

In the free form, curium is a soft silvery-white metal. It exists in two allotropic modiﬁcations:

a low-temperature α-Cm below 873 K, and a high-temperature form β-Cm. The α-Cm variety has a double hexagonal close-packed crystal lattice with alternation of layers according to the 4 ), ABAC. . . scheme; space group P 63 /mmc (D6h a = 0.344 nm, c ≈ 1.16 nm. The β-Cm form has a face-centered cubic lattice, space group F m3m (Oh5 ), a = 0.5039 nm upon hardening. Density of α-Cm is 13.51 g/cm3 ; T melting = 1620 K, T boiling is about 3380 K; speciﬁc heat cp = 27.6 J·mole−1 ·K−1 ; heat of melting is 14.64 kJ/mole, heat of sublimation is 372.6 kJ/mole. Below the Néel point T N = 52 K, α-Cm transforms from the paramagnetic state to the antiferromagnetic one (see Antiferromagnetism); below the critical temperature T c = 205 K, β-Cm is a ferrimagnet, or has a noncollinear magnetic structure. Targets from isotopes 246 Cm and 248 Cm are used in the synthesis of the heavier transuranium elements by bombardment with the multicharged ions. High heat release in the preparations from the isotopes 244 Cm and 242 Cm caused by their α-decay suggests the possibility of using these nuclides to produce small-size nuclear electric current sources that persist for several years (e.g., in onboard space systems). CURRENT CARRIER DRIFT, charge carrier drift

A directed movement of charge carriers in semiconductors under the action of external ﬁelds

imposed on their disordered (thermal) motion. The current density resulting from the charge carrier drift in the electric ﬁeld E (drift current) is j = σ E, where the electrical conductivity σ = e(μe n + μh p), n and p are the concentrations of the conduction electrons and holes, respectively, and μe and μh are their mobilities (see Mobility of current carriers). The total conduction current density is the sum of the drift current, the diffusion current, and the thermoelectric current arising from the presence of a temperature gradient. The charge carrier drift can also result from the carrying along of carriers by either an ultrasonic wave (see Acousto-electric effect) or an electromagnetic wave (radio electric effect, light electric effect). In this event the drift involves nonequilibrium carriers, and therefore it becomes complicated by the

appearance of bulk charges whose ﬁeld should be taken into account in addition to the external ﬁeld and the recombination of current carriers. The motion of injected nonequilibrium carriers (see Injection of current carriers) in the external electric ﬁeld is described by so-called ambipolar mobility μa =

μe μh |n − p| , μe n + μh p

which, in general, differs from μe and μh . For an intrinsic semiconductor n = p and μa = 0; for an n-type semiconductor n p, μa = μh ; and for a p-type semiconductor p n, μa = μe , which means that in an impurity semiconductor μa coincides closely with the mobility of the minority carriers. The velocity of the grouping of nonequilibrium carriers in an external ﬁeld E is equal to μa E. An important characteristic of charge carrier drift is its drift length l, which is the distance that the carriers traverse in going from their point of generation (see Generation of current carriers) to their recombination point. This length has the value l = μEτ , where τ is the lifetime of the nonequilibrium carriers. The method for measuring the drift length is the same as that for measuring the diffusion length. In anisotropic crystals the direction of the drift can differ from that of the electric ﬁeld (since mobilities are tensors). In strong electric ﬁelds the drift can be anisotropic even in isotropic (cubic) many-valley semiconductors. In the presence of a transverse magnetic ﬁeld the drift direction does not coincide with the electric ﬁeld direction. In a strong magnetic ﬁeld B normal to the external electric ﬁeld E satisfying the condition cB E, the charge carriers drift in the direction normal to both E and B with the velocity v = E/B that does not depend on the carrier mobility. A circular motion of the carriers at the cyclotron frequency is superimposed on this drift. CURRENT CARRIER GENERATION See Generation of current carriers. CURRENT CARRIER MOBILITY See Mobility of current carriers. CURRENT CARRIER RECOMBINATION See Recombination.

CURRENT CARRIER SCATTERING

CURRENT CARRIERS, charge carriers Mobile charged particles and quasi-particles.

In an external electric ﬁeld, the random motion of the current carriers acquires a directional component (see Current carrier drift), so that an electric current ﬂows. The current carriers in metals are usually electrons of the conduction band, but when this band is more than half full, the current carrying role is better described in terms of holes in this band. In metals the concentration of current carriers is about 1022 –1023 cm−3 , i.e. is of the order of the number of atoms in the crystal itself, while the mobility μ of conduction electrons usually lies within 105 –107 cm2 ·V−1 ·s−1 ). However, in super-pure metals, it may increase by 3–4 orders of magnitude (see Mobility of current carriers). The carriers of current in semiconductors are usually electrons in the conduction band and holes in the valence band. Their concentrations, n (electrons) and p (holes), may vary by many orders of magnitude from sample to sample of the same material, depending on the concentration of impurity atoms (donors, acceptors), intrinsic defects, the temperature, and external actions. Dark current carriers are those which exist in semiconductors in the absence of photoexcitation; equilibrium current carriers are those present when thermodynamic equilibrium exists between allowed energy bands and local electronic levels. For the case n > p at equilibrium, the majority current carriers are electrons, otherwise they are holes. Nonequilibrium current carriers appear when the electron subsystem is variously excited. The nonequilibrium concentration of minority current carriers may be easily raised far above its equilibrium value. It is controlled by the efﬁciency of the injection of minority current carriers into the band, and by their lifetime in that band. In semiconductors, the mobility of carriers usually lies within the range 102 –104 cm2 ·V−1 ·s−1 . The electron (hole) component of conductivity may include impurity conductivity only, without any input from the allowed band (see Impurity band, Hopping conductivity), and the carrier mobility μ may then remain much lower than 1 cm2 ·V−1 ·s−1 . The interaction of free electrons or holes with the surrounding atoms of the crystal may result in the formation of polarons and ﬂuctuation states of the current carriers (see Polaron, Fluctuon). In insulators the role of charge carriers may be played

263

by interstitial ions of either intrinsic or impurity atoms, or by charged vacancies (see Ionic conductivity). CURRENT CARRIER SCATTERING in crystals A transition of an electron (or hole) between

states described by Bloch wave functions under the action of a perturbation of the periodic crystal e ld. There are two types of such perturbations that inﬂuence the mechanism of the scattering. The ﬁrst type includes static defects of the crystal lattice: impurity atoms, vacancies, dislocations, crystallite boundaries, and the external surface of the specimen (see Surface scattering). The second type includes dynamic perturbations: phonons, other electrons, magnons, etc. The interaction of current carriers with the perturbation of the periodicity is described by a Hamiltonian H = H − H0 , where H is the Hamiltonian of the actual crystal and H0 is the Hamiltonian of an ideal crystal. This results in electronic transitions between the states with quasi-wave vectors k and k and energies ε(k) and ε(k ). Provided |ε(k ) − ε(k)| ε(k) then we have quasi-elastic (elastic) scattering. To each current-carrier scattering mechanism there corresponds a separate Hamiltonian H , a probability W (k, k ) of the transition from state k to state k , and a relaxation time for quasi-momentum τp , provided such a variable may be introduced. Calculations of W (k, k ) are usually carried out within ﬁrst-order perturbation theory (|H | H , the Born approximation), and Δt τp , where Δt is the action time for the perturbation in the elementary scattering event. Scattering hampers directional motions of electrons either in the external electric ﬁeld or under the effect of a temperature gradient, these motions generating the electric current and the energy ﬂux, respectively. The quantity W (k, k ) enters the collision integral in the Boltzmann kinetic equation (see Boltzmann equation), its solution permitting the determination of kinetic coefﬁcients. Among the latter are, in particular, the mobility of current carriers μ and the Hall constant (see Galvanomagnetic effects). The solution of that equation simpliﬁes if the variable τp may be introduced. For the simultaneous action of several scattering −1 mechanisms the values Wi (k, k ) and τpi are

summed: 1/tp = i (1/τpi ). In some cases this

264

CURRENT CARRIER SCATTERING

summation process extends to 1/μ = i (1/μi ) and ρ = i ρi (Matthiessen rule for resistivities ρI ), which hold for τpi independent of k. Provided W (k, k ) depends on the angle between k and k only, the microparticle scattering is called isotropic scattering, and when it also depends on the directions of k and k it is anisotropic scattering. The relaxation time is a tensor in the latter case. Current carrier scattering in semiconductors. Besides the mechanism of scattering proper, this effect is controlled by the dispersion law for the current carriers. When k and k belong to the same valley the process is called intravalley scattering, otherwise it is designated intervalley scattering. If one may express τp ∝ es and μ ∝ T α then the quantities s and α control the scattering process. During the scattering of electrons by lattice vibrations (phonons) a phonon with an energy ω(q) and a quasi-wave number q (ω is the frequency) is either emitted or absorbed in an elementary scattering event. The conservation laws of energy ε(k) = ε(k ) ± ω(q) and quasi-momentum k = k ± q + b are then obeyed. The “minus” sign here corresponds to the absorption of a phonon, while “plus” corresponds to its emission, and b is a reciprocal lattice vector. Processes with b = 0 are the so-called ﬂip-over or Umklapp processes. It is important to account for them when (k − k ) lies outside the ﬁrst Brillouin zone, where b brings q back into the ﬁrst zone. Umklapp processes are insigniﬁcant for valleys in the center of the ﬁrst Brillouin zone (see Many-valley semiconductors). Acoustic vibrations of atoms deform the crystal, changing the energy of the bottom of the conduction band, and produce a scattering acoustic strain potential = ε Δv/v , where ε is the strain potenHac 1 0 1 tial constant (sometimes the strain potential itself), and Δv/v0 is the relative change of a given semiconductor volume, e.g., a unit cell. holds for an The above expression for Hac isotropic electron dispersion law only, and for an extremum at the center of curvature of the ﬁrst Brillouin zone. In the general case the strain potential constant is a tensor (strain potential tensor) to the strain. When T > T = that relates Hac 0 2 mn u /kB ≈ 1 K, where mn is the effective mass of the electron, u is the sound velocity, kB is the

Boltzmann constant, the scattering is quasi-elastic, so that only the phonons with q < 2k take part in it. The Planck distribution function for them may be approximated by the classical expression kB T / that corresponds to an equilibrium energy distribution over the degrees of freedom, so that these are equidistributed phonons. In the simplest case of an isotropic parabolic dispersion law for ε(k) we have s = −1/2, α = −3/2, r = 3π/8 = 1.18. Optical vibrations of atoms produce a scattering optical strain potential (scattering by nonpolar optical phonons). When kB T ω0 , where ω0 is the frequency of an optical phonon, the scattering is elastic, s = −1/2, α = −3/2, r = 3π/8 = 1.18. At all other temperatures the scattering becomes inelastic. Provided, however, that the dispersion law is isotropic (or close to isotropic and averaged over directions), the equality W (k, k ) = W (k, −k ) makes it possible to introduce τp . If kB T ω0 , μ ∝ τp ∝ exp[ω0 /(kB T )], r = 1. Only these two cases of scattering by phonons are possible in nonpolar crystals such as Ge and Si. In polar crystals (e.g., AIII BV ) scattering by the polar optical potential resulting from the lattice polarization (see Polarization of insulator) contributes to the optical vibrations of the atoms (scattering by polar optical phonons). Such scattering may be stronger than scattering from acoustic and optical deformation potentials. It is elastic for kB T ω0 and s = 1/2, α = −1/2, r = 45π/128 = 1.105, and becomes inelastic at other temperatures. However, when kB T ω0 one may introduce τp since electrons can only absorb an optical phonons in a weak electric ﬁeld. Moreover, having absorbed the optical phonon, the electron emits it almost instantaneously (the probability ratio then becomes exp[ω0 /(kB T )] 1. The electron energy undergoes almost no change during such a composite scattering event, while k does change. We have μ ∝ τp ∝ exp[ω0 /(kB T )], r = 1 in the absence of degeneracy. In crystals with partial ionic bonding acoustic vibrations may also produce, beside the deformation potential, a piezoelectric scattering potential, provided the crystal possesses no center of symmetry (e.g., in AIII BV , AII BVI semiconductors, see Piezoelectricity). A piezoelectric constant enters the formulae describing scattering by that

CURRENT CARRIER SCATTERING

potential, and s = 1/2, α = −1/2, r = 45π/128 = 1.105 for the case. At low temperatures the phonon gas is rareﬁed and the main effect may consist in scattering by impurity atoms; the scattering in that case is elastic because of the great difference between the masses of the electron and the atom. Scattering from ionized impurities is similar to the Rutherford scattering of α-particles. The Conwell–Weisskopf formula (E.M. Conwell, V.F. Weisskopf, 1950) obtained for μ for that kind of scattering does not take into account the screening by free electrons of the ﬁeld produced by the impurity ions (see Electric charge screening), while the Brooks– Herring formula does. In both cases, and to within the accuracy of certain factors slowly changing with temperature T and the impurity concentration N , we have τp ∝ e3/2 /N , μ ∝ T 3/2 /N , r = 315π/512 = 1.93. Scattering by neutral impurities is similar to electron scattering by atoms of hydrogen: s = 0, α = 0, r = 1. The corresponding formula for τp is called the Erginsoy formula (C. Erginsoy, 1950). In the case of scattering from point defects with a short-range δ-function potential α = −1.2, s = −1.2. In all the above theories the scattering of current carriers is assumed to be incoherent scattering, with the assumption of no interference between electron waves scattered by different impurity atoms. This is generally true for a random distribution of impurity atoms. The above dependences of the mobility μ on the temperature T are usually not observed experimentally, since they were obtained from idealized models. The reason for such a pronounced disagreement between theory and experiment may lie in a dependence of mn and of the deformation potential on the temperature T . Also, the band may deviate from a parabolic shape, the electrons may exhibit partial degeneracy, etc. For example, in the case of scattering by phonons in germanium, α = −1.66 for electrons and α = −2.33 for holes. Electron–electron scattering does not change the total quasi-momentum of the electron gas, and hence has not affect on either the current or μ. However, provided some other scattering mechanism is simultaneously at work, characterized, as it were, by a τp (ε), both the current and μ will change because of energy redistribution among the electrons. This effect is characterized by the

265

electron–electron scattering time, τee . When the electrons collide with each other, a noticeable exchange of both quasi-momentum and energy takes place, because of the equality of their masses, and τee controls the rate of both processes. In the absence of degeneracy we have τee ∝ n−1 , where n is the electron concentration. The electron–hole scattering is signiﬁcant for high concentrations of current carriers (high temperatures, high levels of injection of electrons). It is similar to scattering by ionized impurities when the ionic charge is opposite to that of the scattered carriers. Scattering by dislocations occurs due to the interaction of current carriers with charged dislocation ﬁlaments, and the deformation potential produced by the ﬁeld of strained dislocations. When the scattering center has a magnetic moment then electron spin- ip scattering becomes possible, which leads to the Kondo effect. The energy relaxation time, τe , may often be represented in the form te ∝ el , where the value of l depends on the scattering mechanism. We have l = −1/2 for the acoustic deformation potential, l = 1/2 for the optical, l = 3/2 for the polar optical, and l = 1/2 for the acoustic piezoelectric potential. The inequality τp τe holds for the averages of τp and τe in the case of quasi-elastic scattering. Scattering of current carriers in metals. This manifests itself in the principal kinetic properties of the metal, its electrical conductivity and thermal conductivity. The electrical resistance is related to the relaxation of the electron quasi-momentum, while the thermal resistance arises from both momentum and energy relaxation. When the momentum relaxation prevails, the Wiedemann–Franz law 2 /(3e2 ), where κ is the elecholds: κ/(σ T ) = π 2 kB tronic thermal conductivity and σ is the electrical conductivity. The scattering of current carriers in metals is also inﬂuenced by the shape of the Fermi surface. In the case of electron–phonon scattering, determining the explicit form of the Hamiltonian H is a difﬁcult problem, since the displacement of ions leads to a signiﬁcant restructuring of the electronic wave functions. At the same time semiempirical techniques are available that make it possible to relate matrix elements of the Hamiltonian to the structure of the Fermi surface. The most well-known one is based on combining the model of rigid (undeformable) ions

266

CURRENT CARRIER SCATTERING

with the pseudopotential method. It is not difﬁcult to demonstrate, without falling back to model considerations, that the squared matrix element of the Hamiltonian H is proportional to the phonon momentum to ﬁrst order for the case of scattering from long-wave vibrations. The mechanism of electron–phonon relaxation depends qualitatively on the relation between the momentum of thermal phonons q and the typical size PF of the Fermi surface (note that an intermediate range PF1 < q < PF2 is also realized in Bi, PF1 and PF2 being the major and the minor semiaxes of the ellipsoidal Fermi surface). Let us introduce the maximum energy of the phonons that can interact with electrons: θ = uPF . The ratio θ/kB in typical metals is of the order of the Debye temperature. At high temperatures we have kB T θ and the phonons with energy of the order of θ and momentum q ≈ PF are important. The number of such phonons and, accordingly, the probability of electron–phonon collisions, are proportional to the temperature T . The electrical resistance is, correspondingly, ρ ∝ T . Since the characteristic energy scale of the change in the Fermi distribution function for electrons (see Fermi–Dirac statistics) kB T is much larger than the phonon energy, such collisions are quasi-elastic, and the Wiedemann–Franz law holds. At low temperatures kB T θ and phonons with energy of the order of kB T and momentum q = kB T /u = PF kB T /θ start to play the decisive role. In this particular case energy relaxation occurs during a single collision event. A signiﬁcant change in the electron momentum ω requires [PF /(q)]2 = [θ/(kB T )]2 collisions. Such a relaxation is essentially a diffusion of electrons over the Fermi surface that proceeds with a typical step of q PF . Due to the laws of conservation of energy and momentum such an electron may only interact with those phonons that have their momenta normal to the electron velocity vector, the number of such phonons being proportional to T 2 . In addition, the squared matrix element of the electron–phonon interaction is proportional to the ﬁrst power, q ∝ T . As a result, the energy relaxation time at low temperatures is te ∝ T −3 , while the transport (pulse) time is proportional to τp ≈ τe [θ/(kB T )]2 ≈ T −5 . The corresponding electrical resistivity follows the Bloch law, ρ ∝ T 5 . Naturally, the Wiedemann–Franz law now no longer

holds. Strictly speaking, the above refers to compensated metals (with equal numbers of electrons and holes), or to metals with open Fermi surfaces. For an uncompensated metal the relaxation of total momentum at low temperatures is controlled by electron–phonon collisions, accompanied by Umklapp processes. Moreover, such processes are only possible in the regions where closed Fermi surfaces come closest to each other, the so-called hot spots or hollows. The transport relaxation time, roughly speaking, is equal to the sum of the time span of transitions across the Fermi surface to one of the hollows by diffusion, plus the time an electron takes to ﬂip over or undergo an Umklapp process in a hollow. Usually the ﬁrst time span signiﬁcantly exceeds the second (Umklapp processes proceed relatively readily), so that the Bloch law remains valid. Umklapp processes may control momentum relaxation only in the range of extremely low temperatures (about 1 K), resulting in an exponential temperature dependence of the electrical resistivity against the background of the predominant inﬂuence of electron–impurity scattering. Electron–electron collisions. Only electrons from regions where the Fermi distribution is blurred or diffuse may take part in such collisions, due to the Pauli principle and the conservation of energy law. In other words, a given electron may only collide with a small fraction of the conduction electrons, of the order of kB T /εF (εF is the Fermi energy), since the number of available states is proportional to kB T /εF . (After one of the electrons enters the diffuse range, another appears automatically, due to energy conservation during their collisions.) Thus, taking into account the Pauli principle lowers the probability of an electron–electron collision by a factor of [εF /(kB T )]−2 (see Fermi liquid). One should also take account of the fact that the screening radius in a typical metal is of the order of the lattice constant, and as a result, the mean free path for electron–electron collisions is lee ≈ a[εF /(kB T )]2 . Umklapp processes during electron–electron collisions are possible when the Fermi surface crosses a plane normal to a certain vector b of the reciprocal lattice located a distance b/4 from the center of the Brillouin zone. The law ρ ∝ T 2 might manifest itself at low enough temperatures when one could neglect the input from

CURRENT STATES IN METALS

electron–phonon scattering, but there is no reliable experimental evidence for this. Meanwhile, electron–electron collisions play a role during the absorption of electromagnetic waves in metals in the near-IR spectral range. Having absorbed an electromagnetic quantum with energy ω kB T the electron may interact with other electrons in a layer of thickness ω. Calculations result in a substitution in the expression for the probability 2 T 2 factor is of electron–electron collisions: the kB 2 2 2 replaced by kB T + [ω/(2π)] . This does not apply at T = 0 where everything is in the ground state. Scattering from static defects is usually elastic, hence the collision probability does not depend on the temperature, and the Wiedemann–Franz law holds. Local defects such as impurity atoms significantly perturb the crystal ﬁeld at distances of the order of a lattice constant a. The ﬁeld of a charged impurity is screened by electrons, the screening radius (Debye radius) in a typical metal also being of the order of a. Therefore, the scattering crosssection is of the order of a 2 , and depends on the relatively weak inﬂuence of the local defects. The mean free path is led ∝ aC −1 , where C is the number of local defects divided by the number of cells in the crystal lattice. CURRENT, CRITICAL See Critical currents. CURRENT, ELECTRIC See Electric current. CURRENT FILAMENTATION, current channeling

Electric current ﬂow in a sample with a nonuniform distribution over the cross-section, i.e. high densities along some channels (ﬁlaments), and low or zero densities along neighboring parallel paths. The phenomenon of current ﬁlamentation may result from an S-shaped current–voltage characteristic. Such a characteristic can arise from certain mechanisms of current carrier scattering in solids. In addition an S-shaped characteristic in a uniform semiconductor may arise from the release of Joule heat (overheating instability); when a temperature increase caused by the current ﬂow leads to additional electron transitions from local electron levels in the conduction band then the current

267

can increase still further, with a further rise in the lattice temperature. The channeling often brings about irreversible processes in the current channel, which could put the device out of operation. If the channeling associated with an S-shaped characteristic happens at high frequencies it may be used for the generation of super-high frequency oscillations (harmonics), as occurs in various types of diodes (e.g., trapped plasma avalanche triggered transit diode, tunnel diode, impact ionization avalanche transit time diode). Besides, the pinch effect may be responsible for current channeling in semiconductors (see Magnetic pressure). Also this channeling may be observed in pure metals at low temperatures through the magnetodynamic mechanism of nonlinearity (see Magnetodynamic nonlinearity). CURRENT, PERSISTENT See Persistent current. CURRENT STATES IN METALS

A hysteresis effect (in an external magnetic ﬁeld B0 ) of electric current rectiﬁcation, and the excitation of a static magnetic moment in the sample when irradiating the latter by an rf (radio wave) of a high amplitude Brf . This takes place at the quasi-static limit ωτ 1 (here ω is the rf frequency; τ is the electron characteristic lifetime) of the anomalous skin-effect, with B0 parallel to the rf magnetic ﬁeld vector Brf . The current states are excited when Brf exceeds a threshold value Bcr ∼ 0.1–1 mT that is determined by ω, the mean free path l, and the character of the electron surface scattering. For diffusion scattering Bcr ∝ ω−1/3 l −2 . In the ideal case of specular reﬂection the current states do not emerge. At the regime of strong nonlinearity Brf > Bcr , the magnetic moment does not vanish even at B0 = 0. For growing Brf , the hysteresis loop approaches a universal curve which is determined only by amplitude Brf , and does not depend on the electrodynamic properties of the metal. The excitation of current states is stimulated by sharp conductivity jumps during the rf period which are due to the appearance and disappearance of trapped electrons in the skin-layer (see Magnetodynamic nonlinearity).

268

CURRENT STATES IN SUPERCONDUCTORS

CURRENT STATES IN SUPERCONDUCTORS

States with a ﬁnite current I at zero voltage which correspond to an inﬁnite electrical conductivity. The current states are metastable under the condition I > Ic where Ic is the temperaturedependent critical current which goes to zero at the transition point Tc . In this case, in the vicinity of Tc , we have Ic = const(Tc − T )3/2 (Bardeen law). The energy E is related with the current as E = Lk I 2 /2, where Lk is the kinetic inductance of the superconductor. Strictly speaking, a current state as a metastable state has a ﬁnite lifetime, but for macroscopic superconducting rings the persistent current decay times are so long that it is reasonable to speak about an “inﬁnite conductivity”. The existence of current states is the consequence of the macroscopic quantum coherence of electronic states of the superconductor which are described by a uniﬁed wave function ψ = F eiϕ . In this case the current state is given by the magnitude of phase gradient ∇ϕ according to j = ns evs , vs =

1 (∇ϕ − 2eA), 2m

where vs is the super uid velocity (velocity of motion of condensate); ns is the temperaturedependent concentration of superconducting electrons (ns /2 is the concentration of Cooper pairs). For a pure superconductor ns = n at T = 0, where n is the total concentration of electrons; for a superconducting alloy with a mean free path l less than the coherence length ξ0 , ns = nl/ξ0 at T = 0. As vs grows, the value ns decreases so that the dependence j (vs ) takes the shape of a curve with a maximum (“depairing curve”). The critical depairing current jc is determined as the maximum of the dependence j (vs ), and is estimated as jc ∼ ns (vs = 0)evc (here vc = Δ/pF is the critical velocity). This estimate gives a critical current density value of jc ∼ 109 A/cm2 which is achieved in thin superconducting ﬁlms or ﬁlaments (with thickness or diameter less than ξ0 ). In bulk samples the depairing current is not reached, as a rule, and the critical current is determined by the decay of the superconductive state via the intrinsic magnetic ﬁeld of the current in type I superconductors (Silsbee rule, F.B. Silsbee, 1916),

N-shaped (left) and S-shaped (right) current versus voltage characteristics.

or by the Abrikosov mechanism of vortex pinning in type II superconductors. The current states also occur at superconducting tunnel junctions (dc Josephson effect). In this case the factor which determines the current through this transition is the phase difference ϕ1 − ϕ2 of the condensate wave functions of the two superconductors: I = Ic sin(ϕ1 − ϕ2 ). CURRENT–VOLTAGE CHARACTERISTIC

The dependence of the electrical current I on the voltage V applied to an electric circuit element. If the element resistance does not depend on the current then the current–voltage characteristic (CVC) is a straight line (Ohm’s law). The I versus V characteristics of some circuit elements can have sections which are nonlinear with various shapes. In semiconductors the appearance of non-linear sections can result from the limitations of current through the contact arising from the dependence of the emission ability of the contact on the presence of regions of space charge, and from the dependence of the current carrier mobility on the electric ﬁeld strength. In some cases a current–voltage characteristic has sections of negative slopes, corresponding to negative resistance dV /dI (see Fig.). Negative resistance means that the conduction occurs under unstable conditions. Fig. left: an I versus V characteristic with an N-shape which is seen in tunnel diodes and in semiconductors containing traps with a speciﬁc dependence of the carrier trapping on their energy. Right: an S-shape characteristic which can result from an “overheating” mechanism, associated with the electron heating, and also from an avalanche breakdown due to impact ionization of impurity atoms.

CYBOTAXIS

CURVATURE TENSOR

Riemann tensor, a 4th rank tensor that characterizes the deviation of the geometry of space from the Euclidean type. The mixed curvature i , is deﬁned through the Christoffel tensor, Rklm i as follows: R i i i symbols Γkl klm = ∂l Γkm − ∂m Γkl + i n n i i Γnl Γkm − Γnm Γkl (here ∂i = ∂/∂x , repeated indices imply summation). The covariant curvature n (where g is the metric tensor Riklm = gin Rklm in tensor) satisﬁes the relations Riklm = −Rkilm = −Rikml = Rlmik ; Riklm + Rilmk + Rimkl = 0. A property of this tensor is that there exists a coordinate system such that the tensor is identically zero when the space is locally Euclidean (i.e. gik may be reduced to the metric tensor of ﬂat space with the corresponding signature via a coordinate transformation in a ﬁnite neighborhood of an arbitrary point). The inverse statement is also valid. Thus, the vanishing of the curvature i provides an invariant criterion for tensor Rklm the Euclidean nature of space that is independent of the choice of coordinate system. This property of the curvature tensor is used in elasticity theory to derive the conditions for the strain compatibility that are equivalent to the vanishing of the curvature tensor formed from the Christoffel symbols which are calculated from the displacement ﬁeld. When the solid contains dislocation and disclination types of defects, which give rise to incompatible deformations, the condition of i = 0 is violated. The solid is compatibility Rklm then internally stressed, i.e. there are tensions in it even in the absence of external loads (see Internal stresses). Such a solid is described by a non-Riemann geometry, with a curvature tensor that differs from zero, and another tensor called n is formed from the Einstein tensor Rkm = Rknm it. Note that Rkm = Bkm , where the so-called “material tensor” Bkm describes the distribution of additional matter that produces incompatible deformations within the body. For example, this relation describes internal stresses in a solid that result from a prescribed density of dislocations (see Dislocation density tensor). CYANIDING

Diffusion saturation of the surface of steel and cast-iron products by nitrogen and carbon simultaneously, generally in melts containing cyanide

269

salts. The thickness of the cyanided layer is 0.05 to 2 mm. Cyaniding increases the surface hardness of the products, their wear resistance, and their endurance limit. Tool steels are cyanided at 450 to 600 ◦ C, structural steels below 950 ◦ C. Cyaniding is distinguished by cementation and nitriding (see Chemical heat treatment) depending on the higher velocity of the process. After the high-temperature cyaniding the products are subjected to hardening and to low-temperature annealing. CYBOTAXIC CLUSTERS Domains with a ﬂuctuation origin having a smectic structure found in a nematic liquid crystal, existing in the vicinity of a nematic–smectic phase transition. Cybotaxic clusters present in the

nematic phase inﬂuence the longitudinal bending and twisting strains. Smectic layers in the cluster should be equidistant. As a result, the Frank elasticity constants K2 and K1 in the neighborhood of the transition in the smectic liquid crystal phase increase directly as the cluster size (see Elasticity of liquid crystals). CYBOTAXIS

Name of a hypothetical three-dimensional arrangement of particles (atoms, molecules) in ﬂuids which are in a state intermediate between one that is completely disordered and one that is crystalline. The term “cybotaxis” was introduced by D. Stewart and R. Morrow (1927). The atoms and molecules in cybotaxes have mobility, but their motion and relative arrangement are not disordered as in the gaseous state. A cybotaxis has no sharply delineated boundary. The lifetime of cybotaxes depends on the composition of the ﬂuid, and the temperature. The basis for introducing the cybotaxis concept was X-ray structure analysis data that reveal that at temperatures slightly above the melting point the arrangement of atoms and molecules in liquids is similar to the arrangement in crystalline solids. It is possible to connect the formation of locally regular clusters in glasses which inherit the structural elements of smelts on quenching, with the presence of cybotaxes in smelts. Cybotaxes are often associated with localized arrangements of molecules in liquid crystals. See also Polycluster amorphous solids, Lebedev crystallite hypothesis, Liquid state models.

270

CYCLIC HEAT TREATMENT

CYCLIC HEAT TREATMENT A heat treatment of metals and alloys involv-

ing periodic heating and cooling of the material. This is employed to induce structural changes that lead to the improvement of mechanical properties. One heating and one cooling event constitute a unit cycle of a cyclic heat treatment. The cycle conﬁguration (i.e. temperature versus time dependence), its parameters (maximum and minimum temperatures of the cycle, heating and cooling rates, exposure time at the maximum temperature of the cycle) and the number of cycles can vary, depending on the type of material being treated, its original condition, and the needed structural changes. A cyclic heat treatment can be carried out so that no phase transitions take place in the temperature range of the cycle. In this case structural changes in the cyclic process account for the plastic deformation due to the thermal stresses which arise as a result of temperature gradients induced by heating and cooling the material. Substantial changes take place in the intragrain dislocation structure, grain interfaces (see Grain boundaries), regions of grains adjacent to interfaces, and the quantity and morphology of particles of phases which gain strength. In particular, the durability of metals and alloys under the conditions of hightemperature creep increases signiﬁcantly. If a cyclic heat treatment involves a phase transition within its temperature range of thermal cycling (e.g., the α ↔ γ transformation in iron and its alloys), the structural changes of a cyclic heat treatment arise as a result of both the plastic deformation caused by thermal stresses and the phase transitions. At low rates of heating and cooling (or for a small difference between Tmax and Tmin ) phase transitions play the main role, and the presence of these transitions can result in the production of tiny uniform sized grains which increase the plasticity and strength of the material. CYCLIC STRENGTH

Resistance to fatigue failure of materials under the application of cyclic loads. Quantitatively cyclic strength may be estimated by the endurance limit. As a rule, cyclic strength is somewhat lower than static strength. First of all, cyclic strength is determined by the maximum cyclic stress and its

amplitude. The greater the average cyclic stress, the lesser the stress amplitude needed for material destruction at the same test base. The character of the stress change between σmax and σmin has a negligible effect on the cyclic strength. That is why cycles of complicated shapes may always be reduced to ordinary ones, and standard fatigue tests are carried out with the use of the simplest cycle conﬁguration. An increase of the cycle frequency, other things being equal, usually gives rise to an increase in the cyclic strength, especially at high temperatures. So long as fatigue cracks are forming from regions of stress concentration on the surface, their state strongly inﬂuences the resulting cyclic strength. As the temperature increases, a shift of fatigue curves towards lower stresses is observed. When temperature changes take place, fatigue disturbances may also arise because of the onset of thermal stresses. Cyclic strength rises with the increase of metal purity with respect to interstitial elements, with the decrease of grain size, and with the formation of a cellular dislocation structure (see Fragmentation). It also depends on the presence and size of the second phase of dispersed particles. The environment in contact with the surface of the crack affects the crack growth due to physicochemical processes taking place at its peak (see Fatigue crack growth). The reliable determination of the cyclic strength is only possible when one takes into account the nature of the product, and the details of the fatigue. CYCLOTRON FREQUENCY, gyromagnetic frequency

Gyromagnetic frequency Ω of charged particle rotation in a constant magnetic ﬁeld B in a plane perpendicular to the ﬁeld. For a free charged particle the cyclotron frequency Ω is determined from the balance of the Lorentz force ev × B by the centrifugal force mv 2 /r, and it is given by Ω = eB/m, where e and m are, respectively, the charge and mass of the free particle, and v = Ωr. The cyclotron frequency determines the energy difference E between the energy levels of a particle in a magnetic ﬁeld: E = Ω. In crystals the motion of particles is more complicated since they interact with the ions of the lattice. In a constant

CYCLOTRON–PHONON RESONANCE

magnetic ﬁeld the energy of the electron (or hole) E and the projection pB of its quasi-momentum p along the direction B are conserved. Hence in momentum space the motion takes place along the intersection of the isoenergetic surface E(p) = E with the plane pB = const. If this curve is closed then the motion is periodic with the frequency Ω = eB/m∗ , where m∗ is the charge carrier cyclotron effective mass. CYCLOTRON PARAMETRIC RESONANCE

Selective absorption of electromagnetic radiation by a semiconductor located at the maximum magnetic ﬁeld of a stationary wave (frequency ω) inside a resonator, when a longitudinal constant magnetic ﬁeld B0 is applied, and the cyclotron frequency Ω is a multiple of half the pump wave frequency ω. Cyclotron parametric resonance is due to instability, arising from time modulation of the electron cyclotron rotation frequency (see Cyclotron resonance). The stabilization of this instability results from nonlinear processes, arising at large electron energies, that lead to a highly nonequilibrium and anisotropic distribution of carriers formed at the cyclotron parametric resonance. The presence of this distribution results in the generation and ampliﬁcation of electromagnetic and acoustic vibrations in semiconductors over a broad frequency range. In a thin sample at cyclotron parametric resonance the electron distribution function is independent of the coordinates. In a bulk semiconductor, when the sample size exceeds the wavelength of the pumping wave in the resonator; then the heterogeneity of the wave magnetic ﬁeld plays an important role. The emerging nonequilibrium distribution becomes rather heterogeneous. It results in gradients of the average energy and concentration, and ﬁnally it gives rise to a static electric ﬁeld Eind (hence a static electromotive force) and a heterogeneous Hall effect with a resonance character. The main cyclotron parametric resonance appears when the cyclotron frequency Ω0 = eB0 /m (e and m are particle charge and mass) is half the modulation frequency ω/2 (Ω0 ∼ ω/2 for linear polarization of the pump ﬁeld in a rectangular resonator, and Ω0 ∼ ω for circular polarization). Cyclotron parametric resonance, like any other parametric resonance of mechanical or electrical vibrations, occurs in resonance zones of instability, and diminishes with the

271

increase of the resonance number n (Ω = nω/2, n = 1, 2, 3, . . .). This resonance can be observed when the electrons make many revolutions in B0 before they collide with other particles and scatter, i.e. Ω0 νl , where νl is the a relaxation rate of the electron pulse. In solids collisions of the conduction electrons with crystal lattice defects (νl = 109 –1011 s−1 ), and scattering by thermal vibrations (electron–phonon interaction) are the most important. The last process limits the observation region of cyclotron parametric resonance: it is at low temperatures (1 to 10 K), where collisions with thermal phonons become rather infrequent. The actually achieved relaxation times provide the lower limit of the frequency region (ω > 109 Hz) where cyclotron parametric resonance can be detected at the ﬁeld value B0 = 0.1 to 1 T. This resonance is a threshold-type effect which can be observed when the pump levels are rather high, i.e. Ω1 > (νe νl )1/2 , Ω1 = eB1 /m, where B1 is the amplitude of the alternating magnetic ﬁeld, and νe is the relaxation rate of the electron energy, νe ≈ (10−4 –10−3 )νl . This condition is valid in ﬁelds B1 ∼ 0.01–0.1 mT. The energy of the resonance particles increases exponentially with time, and can attain large values (electron gas overheating can reach 100 K). It results from the fact that the electron distribution becomes rather nonequilibrium and anisotropic. The energy increase is not inﬁnite, but is limited by nonlinear processes. These are processes such as the nonquadratic spectrum of conduction electrons, which results in the dependence of the mass (and the cyclotron frequency) on the energy, and also affects the energy dependence of the electron relaxation rates. Cyclotron parametric resonance can be used as a method of high-frequency resonance pumping of electrons in conductors to produce an inverted population distribution of charge carrier energies. CYCLOTRON–PHONON RESONANCE

A sharp increase of the electromagnetic wave absorption in semiconductors, when the condition ω = ω0 + nωL is satisﬁed, where ω is the electromagnetic wave frequency, ω0 is the optical phonon frequency, ωL is the Larmor precession frequency, and n is an integer. The resonance is observed at high frequencies (ωτ 1) and in a quantizing magnetic eld (ωL τ 1, ωL kB T ); τ is the

272

CYCLOTRON RESONANCE

time of the electron mean free path. The resonance is associated with transitions of electrons between Landau levels with the simultaneous absorption of a photon and an optical phonon. The singularity of the absorption coefﬁcient at its approach to resonance has a logarithmic nature. Cyclotron–phonon resonance has often been studied experimentally. It is used to determine semiconductor parameters, and in particular the frequency of the optical phonon.

on the Luttinger Hamiltonian matrix. In addition to cyclotron resonance there are spin resonances of free carriers (combined resonance and paramagnetic resonance). These types of absorption, together with the investigation of magnetooptical interband transitions, provide a reliable starting point for understanding energy band structures (see Band theory). CYCLOTRON RESONANCE, ACOUSTIC See Acoustic cyclotron resonance.

CYCLOTRON RESONANCE

Resonant absorption of radiofrequency or microwave energy by an electron or other charged particle in a static magnetic ﬁeld when its gyrofrequency equals the frequency of a perpendicular electric ﬁeld. It corresponds to the diamagnetic resonance absorption of an electromagnetic wave, accompanied by the transition of an electron (or hole) from one stationary orbit to another (mainly, to a neighboring one) in a crystal situated in an external constant magnetic ﬁeld B. By its nature this is an electric dipole resonance. In a solid a charge carrier can move freely longitudinally along B. The transverse motion takes place in a ﬁxed orbit with energy equal to ωc n (in an elementary Brillouin zone with energy E(k) = 2 k 2 /(2m∗ )), where ωc = eB/m∗ is the cyclotron frequency and n is a positive integer (Landau levels). In the case of absorption, the change of carrier energy is ωc for the ground state absorption, and a multiple of ωc for harmonics arising when the dependence E(k) is more complex. The nature of E(k) can be deduced by methods of group theory in solid state physics. A main feature of cyclotron resonance is the possibility of determining the effective mass m∗ directly through a measurement of the absorption frequency. When E(k) is anisotropic then ωc depends on the angle between B and the symmetry axes of the crystal. The main condition for observing cyclotron resonance is the requirement that the conduction electron be able to complete an orbit before colliding (ωτ > 1), where impurities, heterogeneities, and crystal lattice vibrations determine the scattering time τ . For complicated forms of the energy E(k), in particular for the presence of both light and heavy holes in cubic semiconductors, the equations of motion have an obvious classical interpretation. The theory uses a quantum-mechanical calculation based

CYCLOTRON RESONANCE IN METALS, Azbel–Kaner resonance In metals cyclotron resonance amounts to an increase in the high-frequency conductance at fre-

quencies ω which are multiples of the electron cyclotron resonance frequency in a constant magnetic ﬁeld parallel to the sample surface. This phenomenon is due to the repeated synchronous acceleration of electrons during the part of the orbit located within the skin depth δ (see Skineffect). In 1956 M.Ya. Azbel and E.A. Kaner theoretically predicted cyclotron resonance in metals, and E. Fawcett discovered it in Sn and Cu. It has been observed in over 32 metals. The electron acceleration mechanism for cyclotron resonance in metals is as follows (see Fig.). For a magnetic ﬁeld B parallel to the metal surface all electrons move in circular orbits, and periodically with the cyclotron frequency Ω they return to and pass through the skin δ where they are accelerated by the electromagnetic wave. If the resonance condition ω = nΩ, n = 1, 2, 3, . . . , is satisﬁed then the acceleration of the electrons takes place on each cycle of the trajectory, just as it occurs in a cyclotron with a single accelerating region. The skin depth δ in a metal plays the role of the latter. The metal region outside the skin acts as the dees

Cyclotron resonance in metals.

CYCLOTRON WAVES

of the cyclotron. Cyclotron resonance is observed in pure single crystal metals at helium temperatures when the rate of electron collisions is less than Ω. It is observed only for the conditions of the anomalous skin-effect, when the radius of the orbit R and the electron mean free path l are much larger than the skin depth δ. Cyclotron resonance in metals differs significantly from diamagnetic cyclotron resonance in semiconductors. The latter is also called cyclotron resonance when it takes place in a gas-discharge plasma. Diamagnetic resonance occurs in a homogeneous radio-wave ﬁeld. Therefore: (a) it is observed at the fundamental frequency (ﬁrst harmonic) ω = Ω, but not at multiple frequencies, as is the case of cyclotron resonance in metals; (b) it is a maximum when the polarization of the rf electric ﬁeld is perpendicular to the vector B, whereas cyclotron resonance in metals exists at any polarization; (c) it is characterized by a sharp increase of the electromagnetic absorption at resonance, while absorption decreases at cyclotron resonance in metals. The last circumstance is associated with the fact that a sharp increase of the current at cyclotron resonance in metals results in its resonance screening from the the external wave, in the increase of the reﬂection coefﬁcient, and, therefore, in a decrease of the energy absorption. The line shape of cyclotron resonance in metals is rather asymmetric due to the presence of intrinsic cyclotron waves, which have their spectrum localized near harmonics nΩ of cyclotron frequencies. In the case of a nonquadratic electron dispersion law, which is typical for most metals, the cyclotron frequency Ω depends on the value of the electron momentum projection along the direction B, hence it differs for different electrons. In this case cyclotron resonance in metals occurs at the extreme frequencies nΩext , since for electrons with Ωext there is a singularity in the density of states. Owing to the decrease of the resonance electron number the amplitude of the cyclotron resonance in metals decreases, and the lines broaden and become more asymmetric in comparison with the case Ω = const. In so doing the resonance of electrons from the central cross-section, and from the vicinity of special points of the Fermi surface, becomes sensitive to the wave polarization. A small slope of the ﬁeld B relative to the surface leads

273

ﬁrstly to the splitting of the resonance peaks, then to the doubling of their number (Ω = nΩ/2), and to the inversion of the lines. In numerous experiments on cyclotron resonance in metals an important fact has been established: electron scattering on the surface heterogeneities of the sample is almost of the mirror-type. It results in a considerable decrease of the amplitude of the cyclotron resonance in metals, since there arises a new group of electrons sliding along the surface near the mirror boundary of the skin depth. Their contribution to the current is rather more than the contribution of resonance particles, and cyclotron resonance in metals arises from corrections to the smooth nonresonance part of the surface impedance of metals. A complete self-consistent theory of cyclotron resonance in metals at arbitrary reﬂections of electrons from the metal surface over a wide range of frequencies and magnetic ﬁelds has been developed. CYCLOTRON RESONANCE, QUANTUM See Quantum cyclotron resonance. CYCLOTRON WAVES

Intrinsic electromagnetic excitations of degenerate electron–hole solid-state plasmas in a magnetic ﬁeld B. The spectrum of cyclotron waves is localized near the cyclotron resonance frequencies ω = nΩ (n = 1, 2, 3, . . .), for a wave vector k⊥B. Its origin is the collective precession of electrons with the cyclotron frequency Ω, in the absence of magnetic collision-free damping. The distinguishing features of this spectrum are due to the nonlocal properties of the conductivity operator, and depend on the electron dispersion law. For the square law of dispersion there are three independent waves in the vicinity of each cyclotron resonance, namely the ordinary, extraordinary, and longitudinal ones, differing in their spectrum and polarization. The spectrum of the transverse cyclotron waves begins at the point k = 0 from the frequency nΩ, reaches a minimum (about nΩ − Ω/2) at k ∼ R −1 (R is the cyclotron radius), and then asymptotically approaches the initial value nΩ. The attenuation of cyclotron waves is determined by the rate of electron relaxation. Parameters of the Fermi liquid interaction in alkali halides have been measured by cyclotron waves.

This Page Intentionally Left Blank

Dd with different orientation in a unit cell. It is observable by the splitting of bands of absorption and luminescence, the components of which appear to be polarized in orthogonal directions. Davydov splitting happens in the spectra of inorganic crystals with ionic or mixed-type bonds in which one can distinguish groups of strongly bound atoms with different orientation in the lattice (K2 CrO4 , CaWO4 , etc.). Davydov splitting is especially apparent in semiconductors with a layered and chain-like structure (As2 S3 , CdP2 , ZnP2 , etc.) where the unit cell is composed of atoms belonging to two or more translationally inequivalent chains or layers, between which, like in molecular crystals, there is a weak van der Waals bond (see also Fermi–Davydov combined resonance, Van der Waals forces). Davydov splitting in liquid crystals is close in nature to Davydov splitting in crystals with several molecules in the unit cell and is of the order of νe ∼ 10−13 s−1 for electronic transitions or

νv ∼ 10−11 s−1 for vibrational transitions. In liquid crystals, there appears an additional contribution to the splitting, which is associated with the orientation dependence of the dispersion interaction. It is comparable in its magnitude with the Davydov splitting, and observable in impurity absorption bands.

DAMPING, COLLISION-FREE See Magnetic collision-free damping. DAMPING, LANDAU See Landau damping. DANGLING BOND, broken bond An unsaturated covalent bond; a bond from

one atom without a terminus, a kind of structural defect in a solid involving a covalent or ioniccovalent bond. Broken bonds are inherent in both crystalline and amorphous solids (see Amorphous state), and can be arranged in a type of random continuous network; this is common in organic and polymeric glasses (see Vitreous state of matter). Associated with broken bonds in amorphous semiconductors and insulators are features of the electronic spectrum that signiﬁcantly affect the processes of electron transfer and photostimulated phenomena. In many cases broken bonds sufﬁciently high in concentration can be observed with the help of electron paramagnetic resonance since they involve unpaired electrons. The density of broken bonds in amorphous solids can reach 1020 to 1021 cm−3 . Examples of broken bonds are unsaturated bonds of surface atoms. Since the energy can be lowered by saturation (closure) of broken bonds, efforts are made toward surface reconstruction of covalent crystals, and this is an important factor in chemisorption on crystals.

DE BOER PARAMETER (J. de Boer, 1948)

DAVYDOV SPLITTING (A.S. Davydov, 1948)

Ratio of the amplitude of the zero-point vibrations of the atoms in a crystal to the crystal lattice

Splitting of electronic, electronic-vibrational and vibrational states in molecular crystals caused by the presence of inductive coupling between molecules and by the migration of excitation energy in a crystal. Davydov splitting is possible when there are two or more identical molecules

spacing, denoted by ΛB . This provides the stability criterion of the classical crystal state, namely, ΛB 1. However, there are crystals for which ΛB ∼ 1. Since the existence of the crystalline state in such a situation is itself problematic, the deﬁnition of the de Boer parameter should not contain 275

276

DE BROGLIE WAVE

the lattice period. It is determined through the parameters of the pairwise interaction of atoms, parameters of the Lennard-Jones potential. The de Boer parameter for a series of elements has the values: 3 He

4 He

H2 D2 Ne Ar K Xe 0.48 0.43 0.28 0.20 0.09 0.03 0.02 0.01 Crystals for which ΛB ∼ 1 are called quantum crystals. DE BROGLIE WAVE (L. de Broglie, 1924)

The quantum mechanical attribution of wave properties to microparticles (electrons, atoms, molecules, etc.). According to the assumption of L. de Broglie a moving particle with the energy E and momentum p has associated with it a wave with a frequency ν = E/ h and a wavelength λ = h/p. The de Broglie wave length corresponding to the thermal motion of the particles increases with the decrease in temperature T . At a sufﬁciently low temperature when λ becomes comparable to the distance between the particles of a system, then quantum effects begin to play a role (see Quantum liquid, Quantum crystal). DEBYE FREQUENCY See Speci c heat. DEBYE–HÜCKEL THEORY (P. Debye, E. Hückel, 1923)

Thermodynamic theory of electrolytes taking into account the screening of the electrostatic potential (see Electric charge screening) by the mobile ions of the solution. It follows from Debye– Hückel theory that an ion located within the solution is surrounded by a coordination sphere of ions of opposite sign, its radius being l D = # εkB T /(8πe2 I ), where ε is the dielectric constant, I is “ionic force” of the solution, I = (1/2) i ni Zi2 where ni is the concentration of ions of the ith type, and Zi is the valence of the ith ion. The coefﬁcient of activity of the ith ion is equal to exp[−Z+ Z− e2 /(2k B T εl D )], where Z+ , Z− are valences of ions of the corresponding sign of the charge. In the Debye–Hückel theory the possibility of forming a bound pair of oppositely charged ions is also taken into account (in this

case the components of the pair provide the mutual screening). The relation between the concentration of pairs and the concentration of individual screened ions is determined by the total concentration of ions in the solution. This theory is used for the description of defects in nonmetallic crystals, e.g., for the calculation of diffusion coef cients, of ionic conductivity, etc. DEBYE–SCHERRER METHOD, powder X-ray method, polycrystal method (P. Debye, P. Scherrer)

Method of obtaining the diffraction diagram of a polycrystalline material (see Polycrystal) by X-ray scattering. In this method a monochromatic narrow beam of X-rays is incident on a sample in the form of a cylinder or a polished section from a polycrystal. All the crystallites in the sample are assumed to have random spatial orientations, and the Bragg condition is satisﬁed for each set of suitably oriented crystallographic planes. For each allowed crystallite orientation diffracted X-rays will emerge along a cone coaxial with the incident X-ray beam with an aperture angle 4θ , where θ is a Bragg angle (see Bragg law). The result is a family of cones corresponding to diffracted X-rays with various allowed aperture angles 4θ for the various allowed reﬂections. The diffraction picture in the Debye–Scherrer method may be recorded on a cylindrical or ﬂat photographic ﬁlm (debyegram). In the X-ray diffractometry of polycrystalline samples the photographic ﬁlm is replaced by a rotating detector of X-rays. DEBYE TEMPERATURE (P. Debye, 1912) The characteristic crystal temperature Θ D cor-

responding to the Debye frequency ωD (k B Θ D = ωD ), where ωD is the maximum frequency of the crystal lattice vibrations of the crystal (ωD ∝ vs /a, where vs is the sound velocity and a is the crystal lattice constant). In the Debye model the crystal vibration frequencies ω are limited by the Debye frequency (ω ωD ), and the linear dispersion law ω = vs |k| is assumed to be valid, where k is the phonon wave vector which takes on 3N discrete values (N is the number of atoms in the crystal), the largest value of k being π/a. The numerical values of the Debye temperature depend on the atomic mass, and on the strength of the elastic bond between atoms (e.g., for Pb Θ D ∼ 90 K,

DECHANNELING

for diamond Θ D ∼ 2340 K). Knowledge of the value of Θ D allows one to obtain important information about the vibrational spectra of a crystal, and about the characteristics of its chemical bonds. The notion of a Debye temperature is essential for treating the thermodynamics of crystal; it is the approximate temperature boundary which separates the low-temperature (T Θ D ) and high-temperature (T Θ D ) lattice properties of the crystal, where T is the crystal temperature. Using only the single parameter Θ D together with some approximation expressions it is possible to describe the behavior of a whole series of observed physical characteristics of crystals over a broad temperature range below as well as above the Debye temperature. Examples of these are: speci c heat, electrical resistance (Bloch–Grüneisen formula), elastic moduli, Debye–Waller factor for the scattering of X-rays, neutrons, electrons, etc.; properties involving the Mössbauer effect, IR absorption, etc. DEBYE THEORY OF SPECIFIC HEAT See Speci c heat. DEBYE–WALLER FACTOR (P. Debye, I. Waller)

The temperature factor in the expression for the probability of the radiation of photons from crystals, or of elastic processes for the scattering of particles or photons, which takes into account thermal and static displacements of atoms from their sites on a crystal lattice. The Debye– Waller factor is written in the form e−2W , where e−W = exp[iQ(uth + ust )], . . . means double (thermodynamic and conﬁgurational) averaging, and Q is the scattering vector or the wave vector of the radiated photons. If the displacements are counted with respect to the sites of the “average” lattice, W assumes the approximate form W ≈ (1/2)[Q(uth + ust )]2 . In the isotropic approximation 2Wα = (Q2 /3)u2α . For a monatomic crystal, assuming the Debye model, it has the temperature dependence 3Q2 2π 2 T 2 1+ + ··· , 2Wth = 8MkB ΘD 3 ΘD where Θ D is Debye temperature, and T is absolute temperature of the crystal. In the general case Wth . depends on the force constants of the

277

crystal, on the atomic masses and on temperature. The static Debye–Waller factor depends on the elastic constants of the crystal, and on the characteristics of defects (concentration, dimensions, correlation in their location, etc.). Usually Wth 1, and for room temperature W th ∼ 0.01 to 0.1. For impurity atoms, small clusters and dislocation loops W st 1; for dislocations W st 1 and the effects of coherent dissipation disappear in the kinematic approximation; but taking into account the dynamic effects of scattering W st in the case of dislocations requires renormalizing, while, e.g., for the scattering of X-rays the renormalized Debye–Waller factor W st < 1 for a dislocation density less than 105 to 107 cm−3 . The Debye–Waller factor determines the reduction of the coherent scattering intensity I (Q) of X-rays, neutrons and other radiations in crystals: I (Q) = I0 (Q) e−2W , where I0 is the intensity of scattering by the ﬁxed ideal (average) lattice. A Debye–Waller factor also describes the efﬁciency of gamma ray radiation in a crystal without recoil (see Mössbauer effect); in this case it is sometimes called the Lamb–Mössbauer factor. DECA. . . (fr. Gr. δεκα , ten), da

Decimal preﬁx which denotes a 10-fold increase of the value of the basic unit. For instance, 1 dal (dekaliter) = 10 l. DECAY, ISOSTRUCTURAL See Isostructural decay. DECHANNELING Exit from the channelling mode; inﬂuenced by the excitation of phonons, electrons, plasmons,

etc., by the channeling particles. Motion of the channeled particles in the transverse direction can be considered as a drift in the ﬁeld of a random force, caused by deviations from the average continuous potential. In this case the energy of the transverse motion of the channelized ions E⊥ increases in proportion with their movement along the channels (upon reduction of their total kinetic energy), and upon reaching the critical value E⊥c = E0 Ψk the dechanneling occurs; E0 is the initial channelized particle energy, Ψk is the Lindhard angle (see Channeling). The distance at which the density of channeling particles

278

DECI. . .

is reduced by one half is called the dechanneling length. This length for protons with energies from 1 to 10 MeV in silicon lies within the range from 2 to 18 μm. Dechanneling is enhanced by the presence of defects in crystals, especially by impurity or inherent interstitial atoms, located near the axes of the channels, and also by dislocations; in alloys it depends on the degree of ordering, etc. DECI. . . (fr. Lat. decem, ten), d

The decimal fraction preﬁx meaning 1/10 of a particular unit. For instance, 1 dg (decigram) = 0.1 g. DECOMPOSITION OF ALLOYS See Alloy decomposition. DECOMPOSITION, SPINODAL See Spinodal decomposition. DECORATION See Surface decoration. DEEP ENERGY LEVELS AND GREEN’S FUNCTIONS See Green’s functions and deep energy levels. DEEP LEVELS in semiconductors Local electronic levels in semiconductors whose ionization energies are comparable with the band gap width. Deep levels exhibit a diversity of prop-

erties due to their depth, and their physicochemical characteristics. The atoms Zn, Cd, Mn, Fe, Co, and Ni in Si and Ge are double (M2+ ) acceptors; Cu and Ag are triple acceptors, and the impurity Au in Ge produces three acceptor and one donor level. Deep levels are responsible for a series of special electric, optical, photoelectric and other properties in semiconductor materials. The direct introduction of impurities is the main method for obtaining material with the desired properties. Deep level centers possess abnormally large cross-sections for trapping of current carriers, so they can serve as centers of rapid recombination. An attempt to formulate a quantitative theory of deep levels encounters some signiﬁcant obstacles associated with the need for a microscopic description of the defect portion of the crystal and with the multi-electron nature of the problem (i.e. simultaneously taking into account both

the electrons of the defects and the valence electrons of neighboring atoms). For calculating local level parameters given in the literature, various quantum chemical methods are used (see Quantum chemistry of solids), in particular, a Lifshits method of regular perturbations (Green’s functions), a modiﬁed method of effective mass, and some others. These methods are arbitrary in their choice of the periodic ﬁeld potential perturbed by a defect in an ideal crystal, and as a rule are not very accurate. DEFECT

For different varieties see Defects in crystals, Defects in liquid crystals, Anti-Schottky defect, Antisite defect, Antistructural defect, Electrically active extended defects, Frenkel defect, Grainboundary defects, Intrinsic defects, Macroscopic defects, Monopole-type defect, Needle-shaped defect, Planar defect, Rod-shaped defects, Schottky defect, Stacking faults, Stoichiometric defects, Surface defects, Swirl defects, Thermal defects. DEFECT CLUSTERING See Point defect clustering. DEFECT ELASTIC POTENTIAL See Elastic potential of a defect. DEFECT INTERACTION See Elastic interaction of defects, Strain interaction of defects. DEFECTON A quasi-particle which arises from a light defect of a crystal lattice as a result of quantum tunneling (see Tunneling phenomena) through the periodic relief of a crystal. A defecton is characterized by a quasi-momentum which determines its

energy, usually lying within a narrow allowed energy band (defecton band). A vacancion (vacancy wave) in solid helium and an impurity atom of 3 He in crystalline 4 He (impuriton) exemplify defectons. Defectons take part in quantum diffusion which has an unusual temperature dependence, and is very sensitive to the concentration of defects. Due to the small width of the defecton band a non-uniform strain of a crystal brings about the localization of defectons, and their transformation into ordinary point defects.

DEFECTOSCOPY

DEFECTOSCOPY, aw detection

The totality of methods which permit the detection of defects (cracks, pores, gas blisters, extraneous inclusions, liquation, segregation of impurities, etc.) in the structure of a solid. There are several types of defectoscopy. Magnetic defectoscopy records the spreading out of magnetic ﬁelds in the regions of defects, or measures the magnetic properties which change in the presence of defects in the material (ferromagnetic materials or ferromagnetic inclusions in nonmagnetic materials). There are the following variants of magnetic defectoscopy: magnetic-powder method where the scattering ﬁelds are detected at the surface of a magnetized sample of small (several μm) particles of ferromagnetic powders or suspensions (recording is visual); the magneticluminescent method where luminofores are used as powder (particle location recorded using UV radiation); the magnetographic method uses superposition at a ferromagnetic ﬁlm, which is then studied with the aid of a tape-recorder head and an electron-beam indicator; the ferroprobe method using different ferroprobes (in particular, taperecorder heads, magnetic diodes, induction coils, etc.) for recording the scattering ﬁelds. Electrical defectoscopy records the spreading out of the electric ﬁelds near defects, thermal electromotive force, electrical resistance. X-ray defectoscopy detects defects by the variation of the contrast from X-rays passing through the sample. This is applicable to thick samples, and uses photographic ﬁlm or special sensors which record the X-ray intensity at every point of the space, subject it to analysis, and transmit the results to a video device screen. Gamma defectoscopy uses the variation of the intensity of gamma rays passing through the material in the region of defects, and is applicable to thick samples. Beams of high-energy electrons generated by accelerators can detect hidden defects in critical materials. Neutrons can detect defects in massive structures and engineering devices, as well as the concentration of inhomogeneities in ordinary bodies. Defectoscopy based on dynamic light scattering in nematic liquid crystals is used for the

279

control of insulating layers on metal–insulator– semiconductor structures (integrated circuits, conductive plates with dielectric coating, etc.). This method can detect 1 μm pores in insulators, and it provides a nondestructive control of a structure with dielectric insulation, giving information about the type of defects present. The most widespread use of acoustic defectoscopy is the shadow method where the reduction in amplitude or the variation of phase of the incident wave, scattered by the acoustic non-uniformity, is recorded, and the echo-method which measures the time of return of a short acoustic pulse to the piezo-transformer after reﬂection from a defect (see Piezoelectricity). The minimum dimensions of recorded defects and the accuracy of their localization by these methods is of the order of the ultrasound wave length. Also there is a series of special methods for measuring speciﬁc parameters of samples. For instance, the thickness of plates is controlled by the value of their resonance acoustic frequencies, the quality of lamellar structures by their acoustic impedance, and the presence of defects in strongly sound-adsorbing bodies through the spectrum of their free (low-frequency) oscillations. Physico-chemical methods of investigation include the capillary method, luminescent analysis, the chromatic method which employs the interaction of surface-active liquids (see Surfaceactive agents) with defects located at the surface or in regions close to the surface. To investigate microdefects of the structure, the method of etching with subsequent microscopic or electronmicroscope analysis is used (see Electron microscope). Upon the interaction of the crystal surface with a chemically-active medium the points of exposure of the defects, e.g., of dislocations, are “etched” more intensely, and this is then detected by optical or scanning electron microscopy. Dislocations and dislocation loops in foils are detected by transmission electron microscopy. Electron– positron annihilation (see Positron spectroscopy) detects and identiﬁes microdefects due to the ability of positrons to localize and annihilate in the defective areas of the crystal. The processing of positron annihilation spectra or the analysis of their lifetime gives information about the type and distribution of microdefects in crystals. The use of

280

DEFECT RESISTANCE

different types of penetrating radiations and their transformation into optically visible images with the help of special electronic devices called image transformers is a type of defectoscopy. X-rays, γ -quanta, β-radiation of isotopes, beams of highenergy electrons and ions, neutrons, electromagnetic radiation in the range from the near infrared to millimeter and submillimeter waves, are used as penetrating radiations (see Optical defectoscopy). DEFECT RESISTANCE

A property of a material whereby it resists damage and possible failure through the effect of small concentrators of stresses (see Stress concentration). Examples are scratches, small cracks, rough nonmetallic inclusions and other defects, which are fractions of a millimeter in size, i.e. no more than 1 or 2 orders of magnitude larger than the size of a polycrystalline metal grain (see Polycrystal). The defect resistance parameter is a quantitative measure of the defect resistance: D2 = log K v − nτ where K v = R ms /στ is the viscosity coefﬁcient of the metal, R ms is the microspalling resistance, στ is the yield limit, and nτ is the exponent in the parabolic equation governing the initial stage of strain hardening of the metal, σe = Aen (A is a constant, e is the actual strain or deformation): nτ =

log(S v /στ ) , log(ee /eτ )

where S v is the true ultimate strength, ee is the uniform true strain, and eτ is the strain at the yield limit. The criterion of defect resistance D2 = log(σ1 /σi ) (where the ratio σ1 /σi is the rigidity of the state of stress at the vertex of the defect, σ1 is the main normal stress, σi is the intensity of stresses) expresses the condition for the destruction of a metal containing a small defect within an area of low plastic deformation of the magnitude e ≈ 0.02. The parameter of defect resistance as a characteristic of steel toughness supplements the index of fracture toughness (crack resistance), because the latter is not applicable to cracks and defects of submillimeter size. DEFECTS, CONTINUUM THEORY See Continuum theory of defects.

DEFECTS, HEALING See Healing of defects. DEFECTS IN CRYSTALS

Disturbances of the periodicity of atom (ion) positions within a crystal (structural defects). They are subdivided into point, linear, surface (or planar) and bulk types. Point defects are one dimensional imperfections (of atomic scale size) distributed in three dimensions. Examples are vacancies, interstitial atoms and some of their combinations (bivacancies, complexes, etc.), as well as impurity atoms which may be located at regular sites of the crystal lattice (substitutional atom) or between regular sites (doping atom). Unlike other types, point defects can be in thermodynamic equilibrium at the lattice temperature. Linear defects are small in two dimensions, and can have a considerable length in the third. The character of linear defects, and of the displacement ﬁelds created by them, is described by the Burgers contour. This contour may either close on itself or be open, and if it is open then the Bravais lattice vector connecting the starting and ending points is called the Burgers vector. Needleshaped defects characterized by a closed contour are chains of vacancies or interstitial atoms. They are not very stable, and easily decompose by thermally activated or tunnel diffusion of atoms. Dislocations correspond to open Burgers contours. Lattice disturbances which are elongated in two dimensions and small in the third are called surface defects. They form at crystal locations where adjoining lattices differ from one another by space orientation or by atom positionings. Some characteristic types are stacking faults, grain boundaries, and subgrain boundaries (see Subboundaries). Bulk defects are disturbances which are not small in any of their three dimensions. Aggregates of point defects, pores and inclusions of a second phase are included in this type. The inﬂuence of defects on the physical properties of crystals is extremely diverse. It is determined by the character of the binding forces within the crystal, by their energy spectrum (metals, semiconductors, insulators), by the nature of the defects, etc. In semiconductors and insulators, where good electrical, optical or photoelec-

DEFECTS IN PHASE TRANSITIONS

281

tric properties are crucial (see Photoelectric phenomena) point defects play an important role, and dislocations may also make a considerable contribution to the electrical resistance. In construction materials where high strength is essential (see Strength), the role of surface and bulk defects is important. An atmosphere of point defects can strongly inﬂuence the motion of dislocations (see Cottrell atmosphere).

Defects in liquid crystals.

DEFECTS IN LIQUID CRYSTALS

Inhomogeneities of the orientational (see Orientational order) and/or translational ordering of molecules of liquid crystals. Molecular size and macroscopic defects are distinguished. Those of molecular size are formed by additions into the liquid crystal, e.g., molecules of dyes, of ions, of surface-active agents, or as a result of lightor radiation-induced transformations of molecules already present. Macroscopic defects include the following: point defects (hedgehogs, boojums), linear ones (dislocations, linear solitons), planar defects (domain walls) and bulk defects (particlelike solitons). Macroscopic defects are called topologically stable if no continuous transformation is able to transform the ﬁeld of the order parameter to the uniform state. The classiﬁcation of macroscopic defects is based on the calculation of the homotopic groups πi (R) of the space of rank R (region of degenerate states) of the medium. Each class of defects corresponds to an element of the group, identical within the accuracy of continuous transformations of the order parameter; a state without a defect corresponds to the unit defect. This formalism permits one to associate with each class of defects some topological invariant, called the topological charge, which is a generalization of the Burgers vector in the theory of dislocations. The continuous variation of the topological charge of an isolated defect is impossible. In the general case the homotopic group πi (R) classiﬁes a defect of dimensionality d = d − i − 1, where d is the dimensionality of the medium. In a three-dimensional (d = 3) medium group π0 (R) describes walls (i = 0, d = 2), π1 (R) describes lines (d = 1), and π2 (R) describes points (d = 0). The processes of decomposition and merging of the defects are limited by the multiplication law of the group elements. If the group is

Abelian (all elements commute) the result of such processes is always unambiguous, while for a nonAbelian group the result depends on the path along which the decomposition (merging) of the defects occurs. Macroscopic defects cause distortions of the orientation of liquid crystal molecules within the whole volume of the sample. Since it is the orientation of the molecules which determines the distribution of the optical axes (see Director) of the liquid crystal, the defects are easily subjected to investigation by the methods of polarization microscopy (see Optical polarization method). The formation and motion of defects play important roles in practically all processes of the liquid crystal response to external disturbances, such as the stress relaxation, the reconstruction of structure under the effect of an electromagnetic ﬁeld, at phase transitions, etc. As a rule, some topological defects are present even in the equilibrium state of a liquid crystal, and their stability is provided by the boundary conditions (see Fig.). Thus, for example, in a spherical drop of a nematic material (see Nematic liquid crystal) with normal boundary conditions in equilibrium there always exists a point defect within the volume, the hedgehog (Fig., right), and at the tangential lines there are two boojums or surface point defects (Fig., left). Due to the wide variety of defects, and the possibility of performing a broad range of experiments, defects constitute convenient models for the development of topological representations in condensed matter physics (see Topological inhomogeneity). DEFECTS IN PHASE TRANSITIONS

Phase transition defects are of two types, those involving a random local ﬁeld, and those involving

282

DEFECT STRESS SCALE

a random local temperature, depending on their inﬂuence upon the coefﬁcients of the density η(r) or the thermodynamic potential Φ(r) describing the phase transition. Within the phenomenology of the Landau theory, the density in the absence of defects has the form: 2 B D A Φ(r) = η2 (r) + η4 (r) + · · · + ∇η(r) 2 4 2 + · · · − h0 η, (1) where for simplicity the long-range forces are not taken into account, and the one-component order parameter A = A0 (T −T0 ) is included; B, D, A0 are medium constants, and h0 is the external ﬁeld which is conjugated to the order parameter. Point defects of the random local ﬁeld type add the following contribution to Φ(r): hi (r − ri )η(r), (2)

Φh = i

and defects of the random local temperature type lead to the additional contribution 1

ΦT = A(r − ri )η2 (r). 2

(3)

The origin of the terms, defects of random local ﬁeld and random local temperature, is associated with the fact that the “averaged over conﬁguration” values Φ h (r) = hη(r), Φ T (r) = (1/2)Aη2 (r) describe renormalization by the defects of the value of the external ﬁeld h0 and of the phase transition temperature T0 . The local ﬁeld defects bring about strong local distortions of the crystal matrix, because it follows from Eq. (1) that (not too close to T0 ) η(r) ∝ (1/r) exp(−r/r c ) with r 2 c = D/A → ∞ at T → T0 . These defects eliminate the long-range order (see Long-range and short-range order), leading to a complex domain structure in systems with inﬁnitely degenerate η, or to long-term relaxation in systems with ﬁnite degenerate η. Such polarized defects create an average ﬁeld within the crystal, and induce η = 0 at any temperature T , i.e. the phase transition, speaking strictly, is absent (blurred). The random local ﬁeld defects bring about a shift of T0 and lead to anomalies of different physical values in the vicinity of T0 . In the area of similarity theory these defects cause a variation of the

critical indices. The reorienting random local ﬁeld defects are a special class of defects which, unlike frozen defects, bring about an increase in the temperature of pure crystal phase transitions. DEFECT STRESS SCALE See Stress scales of defect structures. DEFECT STRUCTURE ANALYSIS See Microprobe X-ray defect structure analysis. DEFECT SYMMETRY GROUP

This involves both the symmetry of a defect itself as well as the symmetry group of the crystal where the defect appears. Translational symmetry (see Translation) disappears when a single defect is introduced into a crystal. The point group of symmetry of a crystal with a defect reﬂects the symmetry of the point defect, and is a subgroup of the point group of the ideal crystal. If we disregard the crystal distortion induced by a defect then the symmetry of this defect is the same as the symmetry of the site that it occupies. The symmetry groups of the various points of the unit cells for all 230 space groups are given in the International Tables for Crystallography. For an impurity atom (or a vacancy) at a site of a Bravais lattice the defect point symmetry is the same as the crystal point symmetry. The presence of a pair of point defects, dislocation loops in cubic crystals, or particles of a new phase of different symmetry all result in a lowering of the symmetry compared with that of the host crystal. DEFECT THRESHOLD ENERGY See Threshold energy of defect formation. DEFORMATION AT LOW TEMPERATURES See Low-temperature deformation. DEFORMATION BY EXPLOSION See Explosion deformation. DEFORMATION DIAGRAM, stress–strain curve

Graphic representation of the dependence of the deforming force (stress) on the material response (strain). The deformation diagram reﬂects

DEGENERACY

the results of testing solids by different methods such as stretching, compressing, e xure and torsion. As deformation parameters one can select absolute values of elongation, of shearing angle, of torsion angle (see Rod twisting), of deﬂection, or preferably one can work with relative deformations which are ratios of sample dimensions during loading to those before the test. Relative deformations are usually subdivided into two types: a conditional deformation which is the the sum of successive variations of size all relative to the same initial dimension before the test; and a true deformation which is the sum of small variations of size, with each of them relative to the current value of the dimension. The deforming effort is characterized also by either the absolute value of the projection of the force or torsion along some direction (direction of deformation), or by the speciﬁc parameter of stress, i.e. by the force effecting a unit area of some cross-section of the body. The normal stress, namely the component of force perpendicular to the cross-section area, and the tangential stress, due to the projection of the force along (parallel to) the area of the cross-section, are singled out. The stresses are usually divided into conditional and true stresses: the former determined by the relation of the actual force to the initial area of the cross-section, and the latter by the same relation to the current area. To plot a deformation diagram it is possible to use different combinations of the above mentioned deformation and deforming force parameters. For the analysis of physical dependencies of the deformation process the diagram using the coordinates “true deformation–true stress” is the most signiﬁcant. This diagram provides data for the calculation of many basic mechanical parameters of the material (e.g., elastic moduli, yield limit, ultimate strength, strain hardening factor, margin of plasticity). The analysis of a deformation diagram also gives information about the physical mechanisms of plastic deformation, of hardening and of degeneracy. Alternate terminology for a deformation diagram is deformation curve, hardening curve and diagram of loading.

283

tion of temperature, strain, and rate of deformation. The simplest kinetic equation presenting a microscopic description of plastic deformation in terms of the dislocation model of plastic deformation takes the form: ε˙ = bρv, where ε˙ is the rate of deformation, b is the Burgers vector, ρ is the density of mobile dislocations, and v is the mean velocity of their motion. The deformation kinetics is accompanied by an irreversible displacement of dislocations. In addition to the displacement of dislocations, one has to consider the multiplication of dislocations and interactions between them, as well as the effects of other lattice defects, in particular, of disclinations. Two competing processes proceed simultaneously when a crystal is undergoing a deformation: strain hardening and recovery. During hardening the stresses required to maintain a constant rate of deformation increase, while the rate of deformation decreases, if a constant external stress is applied. Recovery decreases the rate of hardening during active deformation (˙ε = const), and produces a steady-state creep under a constant stress. Existing theories describe the deformation kinetics at the ﬁrst stages of deformation, in particular, the appearance of a yield cusp (upper and lower yield limits on the deformation diagram, or stress–strain curve). Still, the deformation kinetics at large plastic deformations cannot yet be unambiguously described in terms of existing theories. DEFORMATION, PLASTIC See Plastic deformation, Discontinuous plastic deformation, Localization of plastic deformation, Plastic twisting deformation, Temperature conditions of plastic deformation. DEFORMATION RATE See Plastic deformation rate. DEFORMATION TENSOR See Strain tensor. DEFORMATION WORK See Work of deformation. DEGENERACY

DEFORMATION KINETICS

The development and interplay of elemental acts of deformation that produce strain in a material. Generally, the strain-inducing stress is a func-

There are two main uses for this term. 1. The ﬁrst use is the presence in a quantummechanical system of several different states which have the same value of some physical quan-

284

DEGENERACY, SPIN

tity, such as energy, angular momentum, etc. The number of such states is called the multiplicity or degeneracy factor. Usually degeneracy is associated with the symmetry of a system; lowering by external factors (ﬁelds) brings about the partial or complete removal of degeneracy, e.g., it leads to the splitting of energy levels (see, e.g., Zeeman effect, Stark effect). 2. The second use of this term concerns the state of a gas of identical particles, whereby their quantum properties become revealed below what is called the degeneracy temperature T0 . For Bose particles (bosons) degeneracy corresponds to Bose–Einstein condensation, and in the case of an ideal Bose gas T0 =

3.32 N 2/3 , mk B (gV )2/3

where N is the number of gas particles, V is the volume, m is the particle mass, and g is the multiplicity. For Fermi particles (fermions) the state of degeneracy corresponds to the almost complete ﬁlling by the particles of states with energies less than the Fermi energy, and to the very low occupancy of higher energy states. For an ideal Fermi gas T0 =

(6π 2 N)2/3 2 . 2mk B (gV )2/3

Conduction electrons in metals (N/V ∝ 1022 to 1023 cm−3 ) are degenerate up to temperatures of about 104 K. In semiconductors with high doping almost complete degeneracy of electrons in the conduction band (or holes in the valence band) can take place at room temperature or below. DEGENERACY, SPIN See Spin degeneracy. DEGENERATE SEMICONDUCTOR A semiconductor with the charge carrier energy distribution described by Fermi–Dirac statistics. The Fermi level is located either within the conduction band or valence band, or is situated in the band gap within ∼k B T from the edge of one

of these bands. Inherent semiconductors become degenerate at high temperatures when k B T becomes comparable to the gap width εg , and when these materials have narrow gaps (HgSe, HgTe)

then one or both types of carrier is already degenerate at room temperature. In doped semiconductors the conduction electrons (holes) become degenerate at high donor (acceptor) concentrations. For high optical excitation or strong injection of charge carriers the degeneracy of nonequilibrium carriers is possible. For an arbitrary degree of degeneracy or multiplicity the thermodynamic and kinetic characteristics of an equilibrium electron–hole semiconductor system are expressed through the Fermi–Dirac integral: ∞ x n dx , Fn (z) = 0 exp(x − z) + 1 where z = ξ/(k B T ), and ξ is the chemical potential. For strong degeneracy, exp[ξ/(k B T )] 1, these formulae are considerably simpliﬁed, and for doped degenerate semiconductors they have the same form as for metals. The degeneracy of charge carriers is especially noticeable in those kinetic effects, which arise from the thermal spread in the energy distribution of the carriers. These include the magnetoresistance effect, electronic thermal conductivity, Peltier effect, Ettingshausen effect, and other effects in semiconductors with isotropic energy spectra (see Thermomagnetic phenomena, Thermoelectric phenomena). In completely degenerate semiconductors at T = 0 K these effects are absent, because, according to the Pauli principle, in transport phenomena only the charge carriers located at or near the Fermi surface and possessing the same energy take part. At T = 0 K these effects are present but they are not appreciable, their value being approximately ξ/(k B T ) or [ξ/(k B T )]2 times (depending on the effect under consideration) less than in non-degenerate semiconductors. The features of degenerate semiconductors are most clearly evident in the presence of quantized magnetic ﬁelds (see De Haas–van Alphen effect, Shubnikov–de Haas effect, Quantum Hall effect, etc.). DEGREE OF ORDER of liquid crystals (V.N. Tsvetkov, 1942)

The quantity which designates the fraction of liquid crystal molecules with their long axes

DE HAAS–VAN ALPHEN EFFECT

285

aligned along the director n. The degree of order S, or the order parameter, is given by the following equation: S=

1 3 cos2 θ − 1 , 2

where θ is the angle between the long axis of an individual molecule and n, and the angle brackets designate averaging over the orientations of the molecules. In the isotropic liquid crystal phase S = 0, for ideal ordering S = 1, and in nematic liquid crystals S ≈ 0.6. The degree of order may be determined, e.g., from NMR spectra. DE HAAS–VAN ALPHEN EFFECT (W. de Haas, P. van Alphen, 1931; predicted by L.D. Landau, 1930)

The oscillating dependence of thermodynamic characteristics of metals, semimetals and degenerate semiconductors on the magnetic ﬁeld B, caused by the quantization of energy levels of the conduction electrons, with a ﬁxed projection of quasi-momentum (pz ) along the direction B = (0, 0, B) (Landau quantization). The de Haas–van Alphen effect is explained in terms of the presence of a selected Fermi energy εF in the spectrum of excitations of an electron Fermi liquid. When the magnetic ﬁeld B is scanned the various n terms of magnetic quantization with the energy En (pz ) and momentum pz in turn intersect εF , and the density of one-electronic states having the energy εF oscillates and passes through a sharp peak each time one of the n curves E = En (pz ) is tangential to the dashed horizontal line E = εF (see Fig.). It is these oscillations which constitute the de Haas–van Alphen effect. Usually the number of terms (N0 ) with energy En < εF is very high: N0 = pF2 /eB (pF is the electron momentum at the energy εF ) and the structure of the de Haas–van Alphen oscillations is determined by the quasi-classical Lifshits–Onsager quantization rules for electrons with an arbitrary dispersion law ε(p) (p is the quasi-momentum) in the magnetic ﬁeld: S(E, pz )/eB = 2π(n + 1/2), n 1. Here S is the cross-section area of the isoenergetic surface ε(p) = E at the plane pz = const. The oscillations are periodic with respect to the reciprocal magnetic ﬁeld with the period

(1/B) = 2πe/S ext , where S ext is the extremal

The curves show the quantum terms in the magnetic ﬁeld En (pz ), and the dashed line indicates the Fermi energy. At T = 0 all the states with En < εF are occupied by electrons, and those with En > εF are all vacant.

cross-section of the Fermi surface ε(p) = εF (the points of extrema En (pz ) and S(εF , pz ) coincide at En = εF ). If the Fermi surface has several extremal cross-sections, then the oscillating parts of the thermodynamic characteristics contain harmonics with periods (1/B), responding to all the extremal areas. The experimental study of the dependence of (1/B) on the direction B gives detailed information about the Fermi surface geometry, and in some cases provides data sufﬁcient for its complete reconstruction. Since the quasi-classic parameter N0−1 is negligible in magnitude the quantum oscillations of the thermodynamic potential of the electronic sys−5/2 . As tem have the relative amplitude A ∝ N0 a rule it is not the potentials themselves that are determined, but rather their derivatives (magnetic susceptibility, compressibility, etc.). In this case A may grow by several orders. At ﬁnite temperatures, T = 0, the boundary of the energy distribution of the electrons is blurred, which reduces the value of A. In the temperature region k B T Ω (Ω is the cyclotron frequency corresponding to the given extremal cross-section of the Fermi surface) the relative amplitude of the lth harmonic is proportional to the exponential factor AT = exp[−2π 2 lk B T /(Ω)]. In addition, the broadening of the electronic terms caused by the electron scattering further reduces A. This effect is taken into account by the so-called Dingle factor AD = exp(−2πlν/Ω), where ν is the reciprocal lifetime of the electronic state, averaged over the extremal cross-section of the Fermi surface. In order to make the factors AT , AD of the order of unity, low temperatures (He range) and

286

DEHARDENING

pure samples are needed. At T → 0 not only do point defects (impurity atoms, vacancies) inﬂuence the value of AD , but also the weak deformational ﬁelds of dislocations, usually unimportant for the kinetics of the conduction electrons. In some cases the contribution of dislocations to AD may dominate. A systematic theory of the de Haas–van Alphen effect was formulated by I.M. Lifshits and A.M. Kosevich (1955). In the presence of magnetic breakdown the de Haas–van Alphen effect is qualitatively more complicated in comparison with the quasi-classical one, but the Lifshits–Kosevich theory can be generalized to this case. DEHARDENING, softening Decrease in strength of a material that had been

brought into a hardened, thermodynamically nonequilibrium state by the effect of some external ﬁeld (temperature, gravitational, mechanical, electric, magnetic, etc.). Such a softening or dehardening proceeds by the transformation of the material into a more stable state with lower energy. Dehardening may occur either during the process of the dehardening action itself (dynamic dehardening) or subsequent to it (static dehardening). To activate the latter in practice the material is usually heated. In the case of crystalline solids dehardening proceeds through the formation, displacement (redistribution) and annihilation of point defects, of linear, surface and volume crystal defects, and their complexes. Depending on the type of defects responsible for the dehardening the latter may exhibit different kinetics, which variously affect the physical and mechanical properties of the material. In most cases dynamic dehardening improves the material plasticity, and only weakly affects the specimen shape as the latter changes under the effect of the external ﬁeld. Dehardening that is related to the formation and spread of cracks lowers the material plasticity. DEHARDENING BY ALLOYING, softening by alloying A decrease of the critical shear strength in metals upon the addition of a small amount of an alloying element (e.g., when alloying tantalum with

rhenium). Dehardening by alloying is observed at

room and lower temperatures when the thermally activated dislocations penetrate the Peierls barriers (see Peierls relief), thereby, to a large extent, determining the value of the critical shear stress. One may relate dehardening by alloying with the lowering of the Peierls–Nabarro strength (see Peierls– Nabarro model). The latter may be explained by the easier formation of double kinks on dislocations at those points where the atoms of the alloying element are located. Dehardening by alloying is also observed when highly active elements are added to body-centered cubic metals. Such elements bond the doping atoms into a second phase, clean the metal matrix, and thus lower the impurity hardening. In that case, the effect of lowering the critical shear stress is observed over a wide temperature range. DELAY LINE, ULTRASONIC See Ultrasonic delay lines. DELTA PHASE (δ -phase)

The fourth allotropic modiﬁcation (see Allotropy) of polymorphous metals (see Polymorphism) (e.g., δ-Mn, δ-Ce), and also solid solutions based on them. Iron is an exception, because the solid solution on its third high-temperature modiﬁcation (see Gamma phase) is called the delta phase or δ-Fe. Like α-Fe it has a body-centered cubic lattice and exists from 1400 ◦ C up to the melting temperature 1540 ◦ C. Alloying iron with elements of Groups III, IV, V and VI broadens the temperature range of the delta phase existence. In some systems (e.g., Fe–Si, Fe–Cr, Fe–P) the stabilization of the δ- and α-phases (see Alpha phase) brings about a merging of their phase regions in their phase diagram. As a result, such phases over their entire temperature range of existence only have a body-centered cubic lattice. This phenomenon is used to create soft magnetic materials (e.g., silicon steels, high-chromium steels, stable against corrosion under stress, etc.). In phase diagrams of other systems, the fourth intermediate phase (counting from the ﬁrst toward the second component) is called the delta phase. In systems with interstitial elements (C, N, etc.) the monocarbides with the NaCl type crystal structure are designated as delta phase.

DEMAGNETIZATION FACTOR TENSOR

DEMAGNETIZATION

A process whereby the magnetization of a magnetic material is reduced. A sample with a magnetic susceptibility located in an externally applied magnetic eld Bapp has a magnetization given by M = (Bapp /μ0 )[χ/(1 + χN)] where N is the demagnetization factor which depends on the sample shape and orientation in the ﬁeld, and can assume values 0 N 1. For an ellipsoidal shape with principal directions x, y, z the corresponding demagnetization factors obey the normalization relation Nx + Ny + Nz = 1, so N = 1/3 in all directions for a sphere. For an ellipsoid of revolution with the external ﬁeld applied along its symmetry axis we have N ≈ 1 − δ for a strongly oblate (diskshaped) sample, and N ≈ δ for a strongly prolate (needle-shaped) sample, where δ 1. This discussion assumes that there is no hysteresis, so that the magnetization M vanishes when the applied ﬁeld is reduced to zero. When hysteresis is present there is partial demagnetization even when there is no shape demagnetization (N = 0) and the external magnetic ﬁeld is lowered to zero. When Bapp reaches zero the remanence Mrem remains (see also Hysteresis). Complete demagnetization in the presence of hysteresis can be achieved in three different ways: 1. Demagnetization by a constant magnetic ﬁeld. After the applied ﬁeld reaches zero it is increased in the reverse direction until it reaches the value −Bc , called the coercive force (coercive ﬁeld). The specimen is now demagnetized to zero (M = 0) in an applied reverse ﬁeld. To completely demagnetize the sample in zero ﬁeld it can be cycled through its hysteresis loop many times with gradually decreasing peak ﬁeld values. 2. Demagnetization by an alternating magnetic ﬁeld. The specimen is subjected to an alternating applied ﬁeld that is gradually diminished to zero from an amplitude that can (or may not) initially exceed Bc . 3. Complete demagnetization by heating. The specimen is heated to a temperature above the Curie point and subsequently cooled in an environment free of any magnetic ﬁelds. DEMAGNETIZATION COOLING See Adiabatic paraelectric cooling.

287

DEMAGNETIZATION FACTOR TENSOR

deﬁning A second-rank symmetric tensor N M between the demagthe relationship H D = −N netization ﬁeld H D and the magnetization vector M of a specimen of permeability μˆ = μ0 (1 + χ) placed in a uniform external magnetic ﬁeld B 0 = μ0 H 0 , where χ = M/Hi is the dimensionless magnetic susceptibility of the material, Hi is the internal ﬁeld, and SI units are being used. The coincides with demagnetization factor tensor N the depolarization factor tensor for a specimen of identical shape and orientation of dielectric constant εˆ placed in a uniform external electric ﬁeld E 0 = D 0 /ε0 . Moreover, all the results valid for the demagnetization factor tensor hold also for the depolarization factor tensor, provided the notations are changed, respectively, from the magnetic to electric case: H → E, B → induction D; permeability tensor μˆ → εˆ ; μ0 M → polarization P ; H D → depolarization ﬁeld E D . The source of the latter ﬁeld lies with the electric charges induced by the applied ﬁeld E 0 at the specimen surface. For a specimen of arbitrary shape the demagnetization factor tensor is coordinate dependent, due to the nonuniform nature of the demagnetization ﬁelds, so its calculation becomes problematic. The most important shape permitting an exact analytic solution is an ellipsoid arbitrarily oriented with respect to B 0 . Within a specimen of that shape the internal ﬁeld values B i , M, and H i = H 0 + H D appear to be uniform, but they may have different directions in space. In the important special case when the principal directions of the tensor μˆ coincide with the ellipsoid principal axes and the applied ﬁeld B 0 is oriented along one of those axes, then the internal ﬁelds B i , M, and H i are all parallel to the applied ﬁeld B 0 . The demagnetization factor tensor is in diagonal form with its principal Ni all positive, obeying the normalization relation

3 N = N + N + N = 1. These demagnetix y z i=1 i zation factors are given by the integral expression: a a a Ni = 1 2 3 2

∞

dq

(ai2 + q)f (q) 0

,

(1)

where f (q) = [(q + a12 )(q + a22 )(q + a32 )]1/2 . For ellipsoids of revolution (a1 = a2 = a3 ) the elliptic integrals (1) reduce to elementary functions.

288

DEMAGNETIZATION FIELDS

The internal ﬁelds are related to the applied ﬁeld through the expression NBi + (1 − N)μ0 Hi = B0

(2)

DEMAGNETIZATION FIELDS Magnetic elds within a magnetic substance

with the following individual values: 1+χ Bi = B0 , 1 + Nχ Hi =

H0 , 1 + Nχ

M=

χH0 , 1 + Nχ

(3)

where B 0 = μ0 H 0 . From symmetry considerations it is clear that N = 1/3 for a sphere. In the limiting cases of an inﬁnitely oblong and oblate ellipsoids of revolution (a long cylinder and a ﬂat disc (plate)), the same considerations yield N = 1/2 for the case when B 0 is normal to the cylinder axis, N = 0 for B 0 parallel to that axis, while N = 1 for B 0 normal to the plate plane. The demagnetization factor tensor is used to calculate internal magnetostatic ﬁelds and also external ﬁelds produced by permanent magnets of various shapes, and likewise for electrostatic calculations. The demagnetization factor tensor plays a signiﬁcant role when determining frequencies of ferromagnetic resonance and ferrimagnetic resonance, and it is important for electron paramagnetic resonance for gμB B/(kB T ) 1, where gμB B is the Zeeman splitting (see Zeeman effect). The demagnetization factor tensor also plays an important role in the theory of the intermediate state of superconductors and magnetic materials in an external magnetic ﬁeld, while the dielectric analogue theory is used to explain the interaction of electromagnetic waves with small particles of various shapes in the Rayleigh approximation (see Rayleigh scattering of light). In the latter case they often introduce a generalization of the concept of depolarization factors, considering particles placed in a medium with the dielectric constant εm > ε0 so that besides the purely geometric factor (1) there appears a dependence on the dielectric properties of both the particle and the medium. If the principal axes of tensors εˆ and N coincide, the generalized factor has the form: i = εi − εm Ni . N εi − ε0 εm /ε0

A generalization similar to (4) may also be introduced for the demagnetization factor tensor with allowance made for the above change in notation.

(4)

(that is either magnetized or placed in an external magnetic ﬁeld), which seek to lower its magnetic moment. The sources of demagnetization ﬁelds are either surface or bulk (ﬁcticious) magnetic charges. To describe demagnetization ﬁelds one traditionally uses the coefﬁcients of the de that relates the demagnetization factor tensor N magnetization ﬁeld H D with a specimen magneM. The value of tization M, so that H D = −N signiﬁcantly depends on the specithe tensor N men shape and may be calculated exactly for an ellipsoidal shape only. In the latter case, both H D remain uniform within the specimen bulk and N is diagonal with the normalizaand the tensor N tion condition Nx + Ny + Nz = 1. For a specimen of an arbitrary shape, its demagnetization ﬁeld is nonuniform. Either empirical or approximate relationships are then used to describe the . When exciting a nonuniform precession tensor N of the magnetization M in a variable magnetic ﬁeld charges form that result in the appearance of variable demagnetization ﬁelds. Such ﬁelds appreciably affect the spectrum of magnetostatic vibrations and waves. DENDRITES (fr. Gr. δενδρoν , tree) Crystals (or aggregations of crystals) of a

branched tree-like conﬁguration. They are formed during crystallization from the melt, solution, vapor, and some metallic glasses. The formation of dendrites is explained by the instability of the source crystal convex shape under the conditions of oversaturation or overcooling of the medium. At the ﬁrst stage projections appear which develop into axes (trunks, ﬁrst-order branches) at which branches of second and higher orders form (see Crystal morphology). The directions of dendrite growth usually coincide with the axis of a pyramid with its sides formed by planes of greatest reticular density: {100} in a face-centered or body-centered cubic lattice, {1010} in a hexagonal close-packed lattice, and {110} in a body-centered tetragonal lattice. In the structures formed by these growths

DENSITY FUNCTIONAL THEORY

(dendrite structure) rounded and faced dendrites are singled out. The former are characteristic of most crystals of pure metals, and of some alloys and organic materials which grow from the alloy and have low melting entropies. Edged dendrites have been found during crystallization from the melt of many nonmetallic materials (semiconductors, oxides, semimetals), and also upon crystallization from vapor and solution. DENSITY

One of the fundamental physical characteristics of a body, which is numerically equal to the mass of a unit volume: ρ = dm/dV , where dm is the mass of a differential element of this substance of volume dV . The mean density of a body is deﬁned as the ratio of the mass of body m to its volume V , i.e. ρ m = m/V . The ratio of the densities of two materials under certain standard physical conditions is referred to as relative density. In the case of porous and loose materials, two types of density are distinguished: true density (not including cavities present in the body) and apparent density (ratio of mass of body to total volume occupied by it). The SI unit for density is kg/m3 , the CGS unit is g/cm3 . As a rule the density increases with increasing pressure and decreases with increasing temperature (due to thermal expansion), except near phase transitions. The value of the density undergoes an abrupt change as a material undergoes a change of state (see States of matter): it sharply decreases upon the transition into the gaseous state, and increases on solidi ca tion (there exists an anomaly in the behavior of the density of water and cast iron: it decreases at the liquid–solid transition). The value of the density of a body is determined by precise determination of the mass and volume of this body by application of various types of densimeters. Also used in density determinations is the dependence of density on the velocity of sound propagation, the intensity of γ and β-radiation passing through a substance, etc. DENSITY FUNCTIONAL, NONLOCAL See Nonlocal density functional. DENSITY FUNCTIONAL THEORY

Method involving a formal, accurate reduction of the problem of the ground state of a many-

289

particle system with strong interactions to a singleparticle problem. Along with Fermi liquid theory and many-particle perturbation theory (method of Green’s functions), density functional theory provides a formalism for explaining many-particle systems. The basis for density functional theory is the Hohenberg–Kohn theorem (P. Hohenberg, W. Kohn, 1964), which states that the energy of a system of interacting fermions (usually electrons) in the ground state is a function of the total particle density only; an external ﬁeld appears in this functional only as the term Vext (r)ρ(r) dr, and the functional minimum in the given ﬁeld corresponds to the true ground state in this ﬁeld. Usually the following energy contributions are explicitly separated out in the density functional: the kinetic energy of noninteracting fermions of the same density ρ(r), the energy of interaction with the external ﬁeld, and the Coulomb (Hartree) energy. The remaining contributions to the energy are called exchange-correlation (Exc ) ones (in the context of many-particle theory this term has a somewhat different meaning; the difference has to do with introduction of part of the kinetic energy into Exc ). To determine the density distribution, which minimizes the above functional, in the form of the density of a certain system of noninteracting particles under the inﬂuence of the effective potential, the effective potential itself is expressed through an externally applied potential, the Hartree potential and the exchange-correlation potential Vxc (r) = δExc {ρ}/δρ(r). The resulting set of self-consistent equations is referred to as the Kohn–Sham equations (W. Kohn, L. Sham, 1965). In the limit of nearly constant density, the local density approximation is valid, according to which Exc = ρ(r)εxc (ρ(r)) dr , where εxc (ρ) is the density of the exchange-correlation energy (see Correlation energy) of the uniform electron gas of density ρ. Most density functional theory calculations are carried out in the context of this approximation. The accuracy of this approximation is quite high for the calculation of observable properties of real solids (equilibrium volume, compressibility, etc.), but there exists a number of problems (e.g., description of the interaction of an electron with a metal surface), which require greater accuracy. Available for application are also nonlocal density functionals, in which

290

DENSITY MATRIX

Exc is an integral function of the electron density in a certain region (mean density approximation, weighted density approximation), and gradient density functionals. The simple expansion, with the gradient-dependent part of Exc proportional to the square of the density gradient, is now rarely used. Widely accepted are Langreth–Mehl processes (D.C. Langreth, M. Mehl, 1983) and the generalized gradient expansion, with its complicated dependence of Exc on the density gradient. Density functional theory may be generalized to treat magnetic systems (spin density functional) at ﬁnite temperatures, and in time-independent external ﬁelds. There exists a relativistic formulation of density functional theory. Density functional theory provides a formal basis for the band theory of solids, since it permits the treatment of the band structure of noninteracting particles under the inﬂuence of an effective periodic potential; the properties of the ground states of this calculated band structure are in full agreement with the properties of the ground states of the crystal under consideration. In combination with band structure computation methods, the density functional theory allows the calculation of the following parameters: equilibrium crystal lattice constants (to an accuracy of several percent), elastic moduli and phonon frequencies (accurate within 10–20%), magnetic moment in magnetic substances (correct to several percent), distribution of electron and spin densities, relative stability of crystal structures, etc. The formulation of density functional theory using the Kohn–Sham equation results in the generation of an additional spectrum which, in general, does not coincide with the actual spectrum of single-particle excitations of the system (since density functional theory is a ground state theory). At the same time, the assumption of a close relationship between these spectra has become the usual practice; this assumption allows one to calculate observed X-ray, optical and other spectra, kinetic characteristics, electron– phonon interaction, etc. Thus, density functional theory provides an opportunity to derive system response functions; in the context of this theory these functions are adequately represented by the above-mentioned additional single-particle spectrum, and the second-order variational derivative

of Exc . The errors involved in calculations of various quantities, based on the local density approximation theory, are (compared to experiment) from several percent (equilibrium lattice constant, magnetic moment of ferromagnets, etc.) to tens of percents for elastic moduli, etc. DENSITY MATRIX, statistical operator (J. von Neumann, L.D. Landau, 1927)

Operator ρ useful for the calculation of the mean value of any physical quantity in quantum statistical mechanics. The density matrix plays the same role in quantum statistical physics as the distribution function does in classic statistical mechanics. Ordinary quantum mechanics deals with systems characterized by a deﬁnite state vector |ψ. The mean value A of any physical in this quantity, represented by an operator A, Quantum-statistical mestate is A = ψ|A|ψ. chanics describes systems that cannot be represented by a state vector, but may be described by giving probabilities W1 , W2 , . . . for existing in states |ϕ1 , |ϕ2 , . . . , respectively. These systems are called statistical mixtures. The mean value in such systems is deﬁned by the formula k , A= Wk ψk |A|ψ Wk = 1, k

k

which may be written in the following contracted form: A = Tr( ρ A), ρ = Wk |ψk ψk |, k

where Tr is the trace of the operator (i.e. sum of its diagonal elements). In order to write the operator ρ in the form of a matrix ρmn in some representation, one has to select an appropriate complete set

of wave functions {|ϕi }. Then

|ψk =∗ i aki |ϕi ρ |ϕn = k Wk akm akn . The and ρmn = ϕm | probability of ﬁnding a system in a (“pure”) state |ϕm from the overall set {|ϕi } is given by the diagonal matrix element ρmm . In the general case, the system is in the “pure” state, if its matrix . To ﬁnd operator satisﬁes the condition ρ2 = ρ the operator ρ , nonequilibrium quantum statistical mechanics uses the quantum Liouville equation (Neumann equation) which plays the same role as the Schrödinger equation for the time evolution of “pure” states (see Quantum kinetic equation). When studying systems that interact with the

DENSITY OF STATES

environment the reduced density matrix is used. It is obtained through averaging the total density matrix of the whole system (quantum system plus environment) over variables of the latter. The reduced density matrix plays an important role in investigating the system response to external disturbances, as well as in studies of such irreversible processes, as transport phenomena, relaxation processes, etc. DENSITY OF ELECTRON STATES

One of the major characteristics of the electron spectrum of solids and other many-electron systems. The density of electronic states g(E) equals the number of electronic states within a unit interval of energy. If the state characterized by quasi-wave vector k in the band λ has the energy Ekλ , then the density of electronic states per unit cell is given by the expression g(E) = (1/N) kλ δ(E − Ekλ ) (see Density of states). If the electron wave functions are expanded in terms of a certain set of basis functions, then the partial densities of electronic states may be introduced, which deﬁne the relative contribution of a given basis function (e.g., orbital state) over a certain energy interval. Of particular importance is the electronic density of states at the Fermi level. It determines kinetic, superconducting, and other properties of a material; and it bears a direct relation to the stability of a crystal lattice and to the thermodynamic properties of electrons. DENSITY OF STATES, spectral density of states

Number of the energy levels of a system per unit energy interval (in more exact terms, the ratio of the number of levels within a certain energy interval to the value of the said interval, when the latter tends to zero). Phonon, electron, magnon, exciton and other densities of states are distinguished in solids. These different types of densities of states correspond to different types of elementary excitation spectra of disordered solids. The density of states determines the spectral (cross-section of absorption and scattering of radio frequency and X-ray radiation, light, neutrons, gamma quanta, ultrasound), thermodynamic (speci c heat, thermal expansion, etc.), and a number of kinetic properties of a material.

291

Of particular importance for metals is the density of electron states at the Fermi surface. Methods of determining the density of states are highly diversiﬁed, and depend on the type of spectrum. Thus, the best results for the phonon and magnon cases of different materials over a wide range of energies are obtained by application of inelastic neutron scattering, whereas the electronic density of states may be determined by employing X-ray photoemission (see X-ray emission spectroscopy). In periodic structures (crystals) the states are described by the quasi-wave vector k, and the energy spectrum is determined by the dispersion law ελ (k), where λ is the number of the spectral band or branch. For these structures, the density of states per unit cell may be represented as 1 δ E − ελ (k) g(E) = N λk

=

ν0 dS , νλ (2π)3 λ

where N is the total number of cells, δ(x) is the Dirac delta function, ν0 is the unit cell volume, and integration with respect to dS is taken over the surface in k -space (within the Brillouin zone), on which ελ (k) = E, and νλ = (1/)|∇k ελ (k)| is the group velocity at this surface. For the case of the phonon spectrum in threedimensional crystals, the spectral density of states behaves as g(E) ∝ E 2 at low values of the energy due to the linear form of the dispersion law (for two-dimensional systems g(E) ∝ E, whereas for one-dimensional ones the density of states is constant in this energy region). Van Hove singularities occur in the density of states in the neighborhood of edges of phonon, electron, and other types of spectra, as well as within the allowed spectral regions, and they feature zero group velocity. In the case of three-dimensional systems, g(E) ∝ (E − Ec )1/2 in the neighborhood of these points, whereas one- and two-dimensional systems show sharper singularities. In imperfect crystals, on the one hand, the density of states peaks in the neighborhood of energies of impurity localized states (see Local electronic levels), which become more and more broadened with increasing concentration of defects, and on the other hand, the smearing of Van

292

DEPLETION

Hove singularities in the neighborhood of spectral edges takes place, and “tails” of the density of states arise in the previously forbidden spectral region. As this takes place, the type of states changes: the continuous spectrum, in which the states are spread throughout the whole crystal (i.e. delocalized) goes over into a spectrum of discrete states, the wave function of which is localized within a limited spatial region. These two types of states are separated by the mobility threshold (see Mobility edge, Anderson localization). The kinetic properties of excitations on different sides of this threshold are quite different, but the density of states in this region remains fairly smooth. At a certain concentration of defects, e.g., impurity atoms of large radius, delocalized states may appear also in the neighborhood of impurity levels. The excitations of low energy in glasses and amorphous compounds (see Amorphous state) are due to quantum transitions between speciﬁc twolevel states (see Two-level systems). The density of states in this case does not tend to zero as it does in the case of ordinary phonon states, but turns out to be constant at low values of energy. This is responsible for the speciﬁc features of the thermodynamic and kinetic properties of these materials at low temperatures (see Low-temperature anomalies in amorphous solids).

DESORPTION

Removal of adsorbed substances from the surface of an adsorbent, a process which is opposite to adsorption. In respect to the effect which causes the desorption the following types are singled out: thermal desorption, electron-stimulated desorption, photodesorption, ﬁeld desorption, and desorption resulting from surface bombardment by fast ions and atoms (cathode scattering). The composition of desorption products may differ from the composition of the adsorbed material. In addition to adsorbed molecules and their parts, molecules chemically bound to the adsorbent may be subjected to desorption. Some material might also accumulate at the adsorbent surface (e.g., carbon during electron-stimulated desorption of carboncontaining adsorbates), or adsorbent material itself might be carried away. DESORPTION COOLING

Process whereby cooling occurs via adiabatic gas desorption. It is carried out by pumpingout the thermoisolated adsorbent (see Adsorption), which has previously adsorbed some quantity of gas. As a result of desorption the temperature of the adsorbent and of the remaining gas is reduced. DESORPTION, ELECTRON-INDUCED See Electron-induced desorption.

DEPLETION of charge carriers

Depletion in a bulk semiconductor (or part of it) of charge carriers due to charge carrier drift in an external electric ﬁeld. Depletion is a phenomenon opposite to accumulation. It occurs in a region adjacent to a potential barrier (e.g., near a semiconductor contact). The barrier limits the amount of carrier ﬂux entering this region. If the carriers depart from it at a high rate due to their drift in an external ﬁeld, the higher the drift rate, the more depleted the region becomes. With a growing ﬁ

Symbol

Numerical value

Speed of light in vacuum Dielectric constant of vacuum Magnetic permeability of vacuum Planck constant

c 7 ε0 = 10 /(4πc2 ) μ0 = 4π·10−7 h = h/(2π) e eV a.u.m. m Mp Mn λ ¯ c = /(mc) a0 = 4πε0 2 /(me2 ) α =λ ¯ c /a0 2 R∞ = /(2ma02 )

2.9979·108 m/s 8.8542·10−12 F/m 1.2566·10−6 H/m 6.6262·10−34 J·s 1.0546·10−34 J·s 1.6022·10−19 C 1.6022·10−19 J 1.6605·10−27 kg 9.1096·10−31 kg 1.6726·10−27 kg 1.6749·10−27 kg 3.8616·10−13 m 5.2918·10−11 m 1/137.036 2.1799·10−18 J 13.605 eV 9.2741·10−24 J/T 5.0508·10−27 J/T 1.3806·10−23 J/K 6.0221·1023 mole−1 8.3145 J·mole−1 ·K−1 1.1605·104 K 2.4180·1014 Hz 1.2398·10−6 m

Elementary charge Electron-volt Atomic unit of mass Electron mass at rest Proton mass at rest Neutron mass at rest Compton wavelength of electrons Bohr radius Fine structure constant Rydberg constant Bohr magneton Nuclear magneton Boltzmann constant Avogadro number Universal gas constant Temperature for kB T = 1 eV Frequency for hν = 1 eV Wavelength for hc/λ = 1 eV

μB = e/(2m) μn = e/(2Mp ) kB NA R = kB N A

CONVENTIONAL UNIT CELLS OF THE 14 BRAVAIS LATTICES

ENCYCLOPEDIC DICTIONARY OF CONDENSED MATTER PHYSICS

This Page Intentionally Left Blank

ENCYCLOPEDIC DICTIONARY OF CONDENSED MATTER PHYSICS

VOLUME 1 A–M EDITED BY

CHARLES P. POOLE JR. Department of Physics and Astronomy University of South Carolina Columbia, SC, USA

2004 Amsterdam – Boston – Heidelberg – London – New York – Oxford Paris – San Diego – San Francisco – Singapore – Sydney – Tokyo

ELSEVIER B.V. Sara Burgerhartstraat 25 P.O. Box 211, 1000 AE Amsterdam The Netherlands

ELSEVIER Inc. 525 B Street, Suite 1900 San Diego, CA 92101-4495 USA

ELSEVIER Ltd The Boulevard, Langford Lane Kidlington, Oxford OX5 UK

ELSEVIER Ltd 84 Theobalds Road 1GB London WC1X 8RR UK

© 2004 Elsevier Inc. All rights reserved. This work is protected under copyright by Elsevier Inc., and the following terms and conditions apply to its use: Photocopying Single photocopies of single chapters may be made for personal use as allowed by national copyright laws. Permission of the Publisher and payment of a fee is required for all other photocopying, including multiple or systematic copying, copying for advertising or promotional purposes, resale, and all forms of document delivery. Special rates are available for educational institutions that wish to make photocopies for non-proﬁt educational classroom use. Permissions may be sought directly from Elsevier’s Rights Department in Oxford, UK: phone (+44) 1865 843830, fax (+44) 1865 853333, e-mail: [email protected]. Requests may also be completed on-line via the Elsevier homepage (http://www.elsevier.com/locate/permissions). In the USA, users may clear permissions and make payments through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA; phone: (+1) (978) 7508400, fax: (+1) (978) 7504744, and in the UK through the Copyright Licensing Agency Rapid Clearance Service (CLARCS), 90 Tottenham Court Road, London W1P 0LP, UK; phone: (+44) 20 7631 5555; fax: (+44) 20 7631 5500. Other countries may have a local reprographic rights agency for payments. Derivative Works Tables of contents may be reproduced for internal circulation, but permission of the Publisher is required for external resale or distribution of such material. Permission of the Publisher is required for all other derivative works, including compilations and translations. Electronic Storage or Usage Permission of the Publisher is required to store or use electronically any material contained in this work, including any chapter or part of a chapter. Except as outlined above, no part of this work may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, without prior written permission of the Publisher. Address permissions requests to: Elsevier’s Rights Department, at the fax and e-mail addresses noted above. Notice No responsibility is assumed by the Publisher for any injury and/or damage to persons or property as a matter of products liability, negligence or otherwise, or from any use or operation of any methods, products, instructions or ideas contained in the material herein. Because of rapid advances in the medical sciences, in particular, independent veriﬁcation of diagnoses and drug dosages should be made. This is a translation from Russian. First edition 2004 Library of Congress Cataloging in Publication Data: A catalog record is available from the Library of Congress. British Library Cataloguing in Publication Data: A catalogue record is available from the British Library. ISBN 0-12-088398-8 volume 1 ISBN 0-12-088399-6 volume 2 ISBN 0-12-561465-9 set ∞ The paper used in this publication meets the requirements of ANSI/NISO Z39.48-1992 (Permanence of Paper).

Printed in The United Kingdom.

EDITOR’S PREFACE TO THE ENGLISH EDITION At the present time Condensed Matter Physics is the largest of the main subdivisions of physics. For several years the Encyclopedic Dictionary of Solid State Physics has been one of the principal reference works in this area, but unfortunately until now it was only available in the Russian language. Its appearance in English is indeed long overdue. It has been a great pleasure for me to undertake the task of editing the English language edition. This two-volume work contains a great deal of material ordinarily not found in the solid state texts that are most often consulted for reference purposes, such as accounts of acoustical holography, bistability, Kosterlitz–Thouless transition, and self-similarity. It provides information on materials rarely discussed in these standard texts, such as austenite, ferroﬂuids, intercalated compounds, laser materials, Laves phases, nematic liquid crystals, etc. Properties of many quasi-particles are presented; for example, those of crowdions, dopplerons, magnons, solitons, vacancions, and weavons. The volumes are fully cross-referenced for tracking down all aspects of a topic, and in this respect we have emulated the excellent cross-referencing systematics of the Russian original. Long lists of alternate titles for looking up subjects can considerably shorten the time needed to ﬁnd specialized information. I wish to thank the members of the Review Panel of the English Language Edition who read over the initial draft of the translation, offered many suggestions and comments for improving the translation, and also provided valuable advice for reﬁning and updating the contents of the articles: Victor Bar’yakhtar, Alexei A. Maradudin, Michael McHenry, Laszlo Mihaly, Sergey K. Tolpygo and Sean Washburn. Thanks are also due to Horacio A. Farach, Vladimir Gudkov, Paul G. Huray, Edwin R. Jones, Grigory Simin, Tangali S. Sudarshin, and especially to Ruslan Prozorov, for their assistance with the editing. The translators did an excellent job of rendering the original Russian text into English, and the desk editor Rimantas Šadžius v

vi

did an outstanding job of checking all the many cross references and the consistency of the notation. The Academic Press Dictionary of Science and Technology has been an invaluable source of information for clarifying various issues during the editing. I wish to thank my wife for her patience with me during the long hours expended in the editing process. The page proofs of this work arrived at my home on the octave day of our 50th wedding anniversary, which we celebrated on October 17, 2003, with our ﬁve children and ﬁfteen grandchildren. Charles P. Poole Jr.

FOREWORD An Encyclopedic Dictionary of Condensed Matter Physics can serve a diverse set of audiences. Professional researchers and university and college teachers interested in learning quickly about a topic in condensed matter physics outside their immediate expertise can obtain the information they seek from such a source. Doctoral students embarking on research in condensed matter physics or materials science can ﬁnd it helpful in providing explanations of concepts and descriptions of methods encountered in reading the literature dealing with their research subject and with related subjects. Undergraduate students with no previous background in condensed matter physics will ﬁnd it a particularly valuable complement to their textbooks as they take their ﬁrst courses in the ﬁeld. Educated laypersons can turn to such an encyclopedia for help in understanding articles published in popular scientiﬁc journals. Until the publication of the Russian edition of the Encyclopedic Dictionary of Solid State Physics, with Professor Viktor G. Bar’yakhtar as its General Editor, no such resource was available to the scientiﬁc community. Its more than 4300 entries were written by more than 700 contributors, specialists in their branches of condensed matter physics, many of whom were well known to an international audience. The task of making this encyclopedia accessible to non-Russian readers was undertaken by Academic Press, with Professor Charles P. Poole Jr. in the role of the General Editor for the English translation. Both the publisher and editor deserve the gratitude of the condensed matter community for bringing this project to fruition. All involved in its production hope that that community will ﬁnd it as useful as its creators intended it to be.

Irvine, California October 29, 2003

Alexei A. Maradudin

vii

This Page Intentionally Left Blank

FOREWORD OF THE EDITORIAL BOARD OF THE ORIGINAL RUSSIAN EDITION This publication is an attempt at a systematized presentation of modern knowledge within all areas of solid state physics from the most fundamental ideas to applied questions. There has been no similar encyclopedic compilation of solid state physics available in the world until now. The Dictionary contains more than 4000 articles. Among them there are relatively long articles devoted to the basic concepts and phenomena of solid state physics, moderate-length articles on particular problems and physical concepts, and, ﬁnally, brief deﬁnitions of terms used in the literature. Considerable attention is paid to technical applications of solid state physics. Brief historical information is given in many articles such as the names of authors and the dates of discoveries. In a number of cases the history of the question is covered in the article. Together with the description of classical topics, special attention is paid to those new ideas that arose only recently in solid state physics and, therefore, often still do not have commonly accepted deﬁnitions. Many articles are provided with illustrations which supplement the text material to help the reader to acquire more complete and more visual information. More than 500 scientists participated in the preparation and the writing of the articles of the Dictionary; these articles were written by specialists working in the particular ﬁelds that they cover. The goal of the publication is to provide needed reference material to a wide audience of readers, which will help them to understand the basic principles of solid state physics. Therefore, the authors endeavored to probe deeply into some salient details of the subject, while preserving a broad perspective throughout the text of the article. The content of articles is interconnected by a system of cross-references. The appended Subject Index will help the reader to orient himself easily in the scope of the various articles. To our deep sorrow, during the period of preparation of the manuscript of this Dictionary, several outstanding scientiﬁc members of the Editorial Board Valentin L’vovich Vinetskii, Yakov Evseevich Geguzin, Emanuil Aizikovich Kaner, Boris Ivanovich Nikolin, Kirill Borisovich Tolpygo, Leonid Nikandrovich Larikov and Alexander Bronislavovich Roitsyn have passed from among us. The recently expired wellknown scientist and prominent publishing specialist Aleksandr Aleksandrovich Gusev, who shared with us his vast knowledge and encyclopedic expertise, provided invaluable aid in the publication of the dictionary. Victor G. Bar’yakhtar, Editor-in-Chief Ernest A. Pashitskii, Vice-Editor-in-Chief Elena G. Galkina, Secretary We started as the team (EDITORIAL BOARD OF THE ORIGINAL RUSSIAN EDITION): V.G. Bar’yakhtar, Editor-in-Cief V.L. Vinetskii, Vice-Editor-in-Chief E.A. Pashitskii, Vice-Editor-in-Chief E.G. Galkina, Secretary

A.S. Bakai Ya.E. Geguzin M.D. Glinchuk Yu.V. Gulyaev ix

B.A. Ivanov M.I. Kaganov E.A. Kaner A.P. Korolyuk

x

A.M. Kosevich L.N. Larikov V.G. Manzhelii

FOREWORD OF THE EDITORIAL BOARD OF THE ORIGINAL RUSSIAN EDITION

B.I. Nikolin A.B. Roitsyn

K.B. Tolpygo M.Ya. Valakh

SCIENTIFIC CONSULTANTS OF THE ORIGINAL RUSSIAN EDITION:

E.M. Baskin E.D. Belokolos L.G. Bugaenko B.M. Bulakh A.V. Chaplik I.M. Dmitrenko V.N. Dobrovol’skii M.I. Dykman B.N. Filippov V.A. Finkel’

V.L. Ginzburg A.V. Golik S.A. Gredeskul V.N. Grigor’yev A.A. Gusev M.A. Ivanov Yu.S. Kaganovskii A.E. Kiv Yu.V. Kornyushin E.N. Korol’

I.O. Kulik O.D. Lavrentovich N.M. Makarov G.D. Mansfel’d Yu.V. Mil’man V.M. Nadutov V.D. Natsyk M.E. Osinovskii L.S. Palatnik

S.S. Rozhkov S.M. Ryabchenko P.V. Ryabko A.V. Sachenko K.K. Shvarts A.A. Slutskin A.I. Sokolov V.A. Tatarenko A.F. Zhuravlev

LIST OF CONTRIBUTORS F.Kh. Abdullaev A.A. Adamovskii S.S. Afonskii I.A. Akhiezer A.F. Akkerman A.B. Aleinikov V.P. Alekhin A.S. Aleksandrov L.N. Aleksandrov B.L. Al’tshuler E.D. Aluker S.P. Anokhov L.I. Antonov K.P. Aref’ev I.E. Aronov M. Ashe Yu.E. Avotin’sh V.G. Babaev Yu.Z. Babaskin S.G. Babich Yu.I. Babii A.S. Bakai Yu.V. Baldokhin O.M. Barabash S.D. Baranovskii Z.V. Bartoshinskii V.G. Bar’yakhtar V.G. Baryshevskii E.M. Baskin F.G. Bass A.N. Bekrenev I.P. Beletskii Ya.A. Beletskii S.I. Beloborod’ko E.D. Belokolos V.F. Belostotskii A.V. Belotskii M.V. Belous

N.P. Belousov K.P. Belov D.P. Belozerov A.I. Belyaeva S.S. Berdonosov B.I. Beresnev L.I. Berezhinskii V.I. Bernadskii I.B. Bersuker V.N. Berzhanskii P.A. Bezirganyan V.F. Bibik I.V. Blonskii E.N. Bogachek A.N. Bogdanov Yu.A. Bogod S.A. Boiko V.S. Boiko S.I. Bondarenko V.N. Bondarev A.S. Borovik-Romanov A.A. Borshch Yu.S. Boyarskaya A.M. Bratkovskii O.M. Braun S.L. Bravina M.S. Bresler A.B. Brik M.S. Brodin V.A. Brodovoi L.T. Bugaenko V.N. Bugaev M. Buikov L.L. Buishvili E.I. Bukhshtab L.N. Bulaevskii B.M. Bulakh A.A. Bulgakov

S.I. Bulychev A.I. Buzdin A.I. Bykhovskii A.M. Bykov Yu.A. Bykovskii G.E. Chaika A.A. Chel’nyi S.P. Chenakin V.T. Cherepin N.F. Chernenko Yu.P. Chernenkov A.A. Chernov S.I. Chugunova B.A. Chuikov K.V. Chuistov A.A. Chumak V.E. Danil’chenko V.D. Danilov L.I. Datsenko A.B. Davydov A.S. Davydov S.A. Dembovskii V.L. Demikhovskii S.A. Demin E.M. Dianov V.V. Didyk I.M. Dmitrenko N.L. Dmitruk V.N. Dneprenko V.S. Dneprovskii V.N. Dobrovol’skii R.D. Dokhner I.F. Dolmanova F.E. Dolzhenkov V.F. Dorfman S.N. Dorogovtsev N.V. Dubovitskaya E.F. Dudnik xi

V.A. Durov V.V. Dyakin M.I. Dykman A.I. Eﬁmov A.L. Efros Yu.A. Ekmanis M.A. Elango V.M. Elinson P.G. Eliseev V.A. Elyukhin Yu.P. Emets V.V. Emtsev V.Z. Enol’skii I.R. Entin I.R. Entinzon E.M. Epshtein A.I. Erenburg A.S. Ermolenko E.D. Ershov A.M. Evstigneev M.I. Faingol’d V.M. Fal’chenko V.L. Fal’ko B.Ya. Farber M.P. Fateev I.M. Fedorchenko O.P. Fedorov A.G. Fedorus Ya.A. Fedotov I.V. Fekeshgazi A.V. Filatov B.N. Filippov V.A. Finkel’ V.M. Finkel’ A.Ya. Fishman N.Ya. Fogel’ E.L. Frankevich L.I. Freiman

xii

V.M. Fridkin I.Ya. Fugol’ B.I. Fuks A.M. Gabovich S.P. Gabuda A.Yu. Gaevskii Yu.A. Gaidukov V.P. Galaiko R.V. Galiulin Yu.M. Gal’perin M.Ya. Gamarnik G.D. Gamulya E.M. Ganapol’skii V.G. Gavrilyuk Ya.E. Geguzin B.L. Gel’mont D.S. Gertsriken I.A. Gilinskii I.A. Gindin S.L. Ginzburg E.I. Givargizov E.I. Gladyshevskii A.A. Glazer L.I. Glazman A.I. Glazov M.D. Glinchuk E.Ya. Glushko V.M. Gokhfel’d V.L. Gokhman V.A. GolenishchevKutuzov A.V. Golik M.F. Golovko T.V. Golub D.A. Gorbunov L.Yu. Gorelik Yu.I. Gorobets V.I. Gorshkov V.V. Gorskii V.G. Grachev S.A. Gredeskul V.P. Gribkovskii P.P. Grigaitis V.N. Grigor’ev O.N. Grigor’ev Yu.M. Grin’ V.V. Gromov V.V. Gudkov A.V. Gulbis

LIST OF CONTRIBUTORS

A.P. Gulyaev Yu.V. Gulyaev M.E. Gurevich Yu.G. Gurevich K.P. Gurov R.N. Gurzhi M.B. Guseva A.N. Guz’ V.M. Gvozdikov A.I. Ignatenko V.V. Il’chenko E.M. Iolin I.P. Ipatova S.S. Ishchenko Z.A. Iskanderova V. Iskra V.G. Ivanchenko P.G. Ivanitskii A.L. Ivanov B.A. Ivanov M.A. Ivanov N.R. Ivanov G.F. Ivanovskii P.F. Ivanovskii V.G. Ivantsov R.K. Ivashchenko O.M. Ivasishin Yu.A. Izyumov G.A. Kachurin A.N. Kadashchuk A.M. Kadigrobov M.I. Kaganov E.B. Kaganovich Yu.M. Kaganovskii N.P. Kalashnikov P.A. Kalugin G.G. Kaminskii E.A. Kaner L.N. Kantorovich A.S. Kapcherin A.A. Kaplyanskii A.L. Kartuzhanskii A.L. Kasatkin V.N. Kashcheev N.I. Kashirina G.A. Katrich B.V. Khaenko I.B. Khaibullin V.A. Kharchenko

E.I. Khar’kov S.S. Khil’kevich A.I. Khizhnyak G.E. Khodenkov A.R. Khokhlov G.A. Kholodar’ V.A. Khvostov K.I. Kikoin S.S. Kil’chitskaya O.V. Kirichenko A.P. Kirilyuk P.S. Kislyi A.E. Kiv Ya.G. Klyava V.M. Knyazheva E.S. Koba L.S. Kogan V.V. Kokorin Yu.A. Kolbanovskii G.Ya. Kolbasov A.G. Kol’chinskii V.L. Kolesnichenko V.V. Kolomiets V.I. Kolomytsev E.V. Kolontsova V.G. Kon A.A. Konchits S.N. Kondrat’ev M.Ya. Kondrat’ko V.A. Kononenko V.I. Konovalov A.I. Kopeliovich V.A. Koptsyk T.N. Kornilova Yu.V. Kornyushin E.N. Korol’ N.S. Kosenko A.M. Kosevich O.G. Koshelev A.S. Kosmodamianskii E.A. Kotomin N.Ya. Kotsarenko Yu.N. Koval’ V.V. Koval’chuk A.S. Kovalev O.V. Kovalev M.Yu. Kovalevskii Yu.Z. Kovdrya I.I. Kovenskii

V.I. Kovpak V.I. Kovtun A.V. Kozlov N.N. Krainik V.V. Krasil’nikov A.Ya. Krasovskii L.S. Kremenchugskii V.P. Krivitskii M.A. Krivoglaz V.N. Krivoruchko A.A. Krokhin S.P. Kruglov I.V. Krylova A.Yu. Kudzin L.S. Kukushkin I.O. Kulik V.A. Kuprievich A.I. Kurbakov A.V. Kurdyumov V.G. Kurdyumov G.G. Kurdyumova M.V. Kurik M.I. Kurkin N.P. Kushnareva V.A. Kuz’menko R.N. Kuz’min V.N. Kuzovkov A.I. Landau V.F. Lapchinskii L.N. Larikov F.F. Lavrent’ev O.D. Lavrentovich B.G. Lazarev L.S. Lazareva Ya.S. Lebedev B.I. Lev A.P. Levanyuk A.A. Levin I.B. Levinson V.A. Likhachev M.P. Lisitsa V.M. Lisitsyn V.A. Lisovenko F.V. Lisovskii P.G. Litovchenko V.G. Litovchenko V.S. Litvinov V.A. Lobodyuk V.M. Loktev V.F. Los’

LIST OF CONTRIBUTORS

D.V. Lotsko V.P. Lukomskii G.A. Luk’yanov V.A. L’vov S.N. Lyakhimets V.G. Lyapin B.Ya. Lyubov I.F. Lyuksyutov R.G. Maev V.M. Maevskii L.L. Makarov N.M. Makarov V.I. Makarov D.N. Makovetskii L.A. Maksimov V.V. Malashenko B.Z. Malkin G.D. Mansfel’d V.G. Manzhelii V.G. Marinin S.V. Marisova V.Ya. Markiv Yu.V. Martynenko T.Ya. Marusii S.V. Mashkevich V.S. Mashkevich T.V. Mashovets V.V. Maslov O.I. Matkovskii Z.A. Matysina V.F. Mazanko I.I. Mazin E.A. Mazur B.V. Mchedlishvili M.V. Medvedev V.K. Medvedev A.I. Mel’ker G.A. Melkov V.S. Mel’nikov F.F. Mende Yu.Ya. Meshkov G.A. Mesyats V.P. Mikhal’chenko V.S. Mikhalenkov V.V. Milenin V.K. Milinchuk Yu.V. Mil’man M.G. Mil’vidskii V.N. Minakov

xiii

E.V. Minenko D.N. Mirlin I.A. Misurkin V.Ya. Mitrofanov N.V. Morozovskii V.V. Moshchalkov N.P. Moskalenko S.A. Moskalenko V.N. Murzin V.P. Naberezhnykh T.A. Nachal’naya V.M. Nadutov E.L. Nagaev V.E. Naish N.G. Nakhodkin V.D. Natsyk A.G. Naumovets O.K. Nazarenko E.I. Neimark I.M. Neklyudov I.Yu. Nemish V.V. Nemoshkalenko S.A. Nepiiko V.A. Nevostruev S.A. Nikitov M.Yu. Nikolaev B.I. Nikolin A.B. Nikol’skii G.K. Ninidze A.I. Nosar’ N.N. Novikov N.V. Novikov V. Novozhilov S.G. Odulov V.I. Okulov E.F. Oleinik N.V. Olechnovich S.I. Olikhovskii B.Z. Ol’shanetskii A.N. Omel’yanchuk A.N. Orlov S.P. Oshkaderov M.E. Osinovskii S.S. Ostapenko E.L. Ostrovskaya D.E. Ovsienko R.P. Ozerov G.A. Pacharenko P.P. Pal’-Val’

S.V. Panyukov I.I. Papirov E.S. Parilis A.M. Parshin E.A. Pashitskii L.A. Pastur R.E. Pasynkov E.P. Pechkovskii G.P. Peka V.I. Peresada S.P. Permogorov V.G. Peschanskii I.S. Petrenko E.G. Petrov V.A. Petrov Yu.N. Petrov G.A. Petrunin V.Yu. Petukhov A.S. Pikovskii G.E. Pikus A.N. Pilyankevich V.I. Pipa F.V. Pirogov G.S. Pisarenko E.A. Pisarev L.P. Pitaevskii A.B. Plachenov B.T. Plachenov Yu.N. Podrezov A.E. Pogorelov V.Z. Polinger Yu.N. Polivanov V.V. Polotnyuk S.S. Pop Yu.M. Poplavko L.E. Popov V.E. Pozhar L.I. Pranyavichus A.I. Prikhna V.E. Primachenko V.G. Prokhorov G.I. Prokopenko P.P. Pugachevich V.V. Pustovalov V.I. Pustovoit A.P. Rachek V.A. Rafalovskii V.V. Rakitin E.I. Rau

B.S. Razbirin A.R. Regel’ V.R. Regel’ V.Yu. Reshetnyak Yu.Ya. Reutov I.S. Rez I.M. Reznik Yu.A. Reznikov D.R. Rizdvyanetskii A.B. Roitsyn O.V. Romankevich A.E. Romanov A.S. Rozhavskii S.S. Rozhkov V.V. Rozhkov E.Ya. Rudavskii A.V. Rudnev I.N. Rundkvist S.M. Ryabchenko P.V. Ryabkov K.P. Ryaboshapka V. Rybalka A.I. Ryskin V.I. Ryzhkov A.M. Sabadash V.A. Sablikov A.V. Sachenko M.V. Sadovskii O.G. Sarbei V.M. Schastlivtsev Yu.V. Sedletskii S.I. Selitser A.V. Semenov Yu.G. Semenov A.I. Senkevich T.N. Serditova T.N. Sergeeva S.E. Shafranyuk S.I. Shakhovtsova A.M. Shalaev B.N. Shalaev B.D. Shanina B.Ya. Shapiro I.G. Shaposhnikov O.D. Shashkov V.G. Shavrov D.I. Sheka V.I. Sheka R.I. Shekhter V.A. Shenderovskii

xiv

S.I. Shevchenko A.Ya. Shik V.B. Shikin Yu.M. Shirshov S.V. Shiyanovskii G.N. Shkerdin O.A. Shmatko A.S. Shpigel’ T.D. Shtepa E.I. Shtyrkov Yu.N. Shunin A.K. Shurin K.K. Shvarts E.A. Silin’sh A.F. Sirenko A.I. Sirko A.A. Sitnikova F.F. Sizov E.V. Skokan V.V. Skorokhod V.V. Sleptsov A.A. Slutskin A.A. Smirnov L.S. Smirnov G.A. Smolenskii O.V. Snitko V.I. Sobolev A.I. Sokolov I.M. Sokolov A.S. Sonin E.B. Sonin A. Sorokin M.S. Soskin A.L. Sozinov V.B. Spivakovskii I.E. Startseva A.N. Starukhin E.P. Stefanovskii M.F. Stel’makh I.A. Stepanov I.A. Stoyanov

LIST OF CONTRIBUTORS

M.I. Strashnikova V.I. Strikha V.I. Sugakov A.P. Sukhorukov S.V. Svechnikov V.M. Svistunov I.I. Sych A.K. Tagantsev G.A. Takzei A.P. Tankeev V.V. Tarakanov V.V. Tarasenko G.G. Tarasov Yu.V. Tarasov I.A. Tarkovskaya V.A. Tatarchenko V.A. Tatarenko I.I. Taubkin V.A. Telezhkin Yu.S. Tikhodeev L.V. Tikhonov E.A. Tikhonova B.L. Timan S.F. Timashev B.B. Timofeev V.B. Timofeev Yu.A. Tkhorik K.B. Tolpygo S.K. Tolpygo P.M. Tomchuk V.I. Tovstenko V.I. Treﬁlov O.A. Troitskii V.A. Trunov V.A. Tsekhomskii B.E. Tsekvava R. Tsenker B.S. Tsukerblat V.M. Tsukernik L.T. Tsymbal N.V. Tsypin

L.I. Tuchinskii A. Tukharinov E.A. Turov Yu.D. Tyapkin V.M. Tyshkevich V.A. Tyul’nin K.M. Tyutin A.A. Urusovskaya A.I. Ustinov B.K. Vainshtein S.B. Vakhrushev M.Ya. Valakh V.I. Val’d-Perlov A.A. Varlamov I.A. Vasil’ev L.I. Vasil’ev M.A. Vasil’ev F.T. Vas’ko A.V. Vedyaev B.G. Vekhter O.G. Vikhlii V.L. Vinetskii E.A. Vinogradov B.B. Vinokur V.M. Vinokurov Yu.P. Virchenko A.S. Vishnevskii I.M. Vitebskii N.A. Vitovskii V.I. Vladimirov V.V. Vladimirov N.A. Vlasenko A.D. Vlasov K.B. Vlasov O.G. Vlokh E.D. Vol A.F. Volkov P.Yu. Volosevich V.A. Voloshin V.D. Volosov S.V. Vonsovskii

D.L. Vorob’ev S.A. Vorob’ev Yu.V. Vorob’ev A.M. Voskoboinikov B.E. Vugmeister D.A. Yablonskii Yu.N. Yagodzinskii L.N. Yagupol’skaya Yu.I. Yakimenko B.I. Yakobson M.V. Yakunin V.A. Yampol’skii I.K. Yanson A.M. Yaremko A.A. Yatsenko A.F. Yatsenko I.A. Yurchenko Yu.F. Yurchenko P.A. Zabolotnyi V.A. Zagrebnov Yu.R. Zakis E.Ya. Zandberg I.M. Zaritskii E.V. Zarochentsev I.K. Zasimchuk E.E. Zasimchuk S.S. Zatulovskii E.A. Zavadskii P.Yu. Zavalii Yu.S. Zharkikh I.S. Zheludev G.N. Zhizhin A.F. Zhuravlev S.N. Zhurkov O.S. Zinets D.N. Zubarev M.D. Zviadadze L.O. Zvorykin B.B. Zvyagin I.P. Zvyagin

INTRODUCTION 1

We introduce to the reader the Encyclopedic Dictionary of Solid State Physics . This Dictionary was planned several years ago, and the aim of its compilers was not only to provide a wide audience of readers with comprehensive and detailed information about different processes, phenomena, and effects in the solid state, but also to enlarge our understanding of the modern terminology in which this information is presented. The latter was very important for the compilers, since they were united by the idea that the achievements of solid state physics during recent decades were due not only to the fantastic development of experimental techniques and the level of experimental skill, but were also due to the creation of a uniﬁed system of concepts and terms adequately reﬂecting the observed regularities and the depth of understanding of the physical processes taking place in solids. The balanced rhythm of the modern language of solid state physics is determined by the theory of symmetry. It governs all theoretical constructions and the coefﬁcients of the equations describing equilibrium and near-equilibrium states of a solid. The dynamic theory of a crystal lattice in the harmonic approximation, which is based on the discrete symmetry of ordered atomic arrangement in a crystal, is a classical example how symmetry considerations are utilized. Another “hidden” symmetry is used, e.g., to describe a number of properties of magnetic, ferroelectric, and superconducting materials. A particular kind of symmetry based on the regularities in diverse phase transitions is apparent in modern scaling theory. The reader will ﬁnd applications of the theory of symmetry in many of the articles. The majority of the phenomena of recent interest in solids were associated with low-level excited states of a substance. It appeared that while atoms or molecules are structural elements of a crystal lattice (and, generally, of any condensed state of a substance), certain collective excitations are the elements of every type of motion (elements of dynamics) in a solid. In view of the macroscopic homogeneity of the unbounded model of a solid, or the periodicity of an unbounded crystal lattice, such collective motions must take the form of plane waves, with a dispersion law that satisﬁes strict symmetry requirements. The quantization of elementary excitations leads to the image of a “corpuscle”, or a quasi-particle. The concept of a quasi-particle and the idea of almost ideal quantum gases composed of various quasi-particles, enrich the language of solid state physics and allow one, within a uniﬁed system of terms and concepts, to treat physical phenomena that are quite diverse and have, at ﬁrst glance, little in common. Therefore, it is not surprising that in the articles devoted to phonons, magnons, excitons, and to electrons or polarons as well, we ﬁnd very similar equations and conclusions. The universality of the physical language reﬂects the unity of Nature itself. The passage to the study of highly excited states of a material led to the creation of the nonlinear dynamics of solids. New contributions to the lexical reserve of the language of solid state physics originated from nonlinear dynamics. For example, the concepts of topological and dynamic solitons were put forward, dynamic solitons appearing in solid state physics as a new type of collective excitation of a condensed medium. Not all parts of solid state physics are presented here with the same completeness and the same amount of detail. The branches reﬂecting the scientiﬁc interests of solid state physicists from the Ukraine and other former Soviet Union republics are the most extensively described. Although general problems of solid state 1

This is the title of the book in Russian (Editor’s note). xv

xvi

INTRODUCTION

physics are less systematically presented, the following areas are covered rather deeply and broadly: physical properties of metals, including superconductivity, electrical and optical properties of semiconductors and insulators, magnetism and magnetic materials, mechanical properties of crystals, and physics of disordered systems. One may also notice an emphasis on the applied physics of plasticity and strength. This is because of the fact that, although physics is an objective international science, some of its presentations or overviews found in textbooks, monographs, or encyclopedic publications unintentionally introduce subjective ideas and personal preferences of authors. The Dictionary includes articles reﬂecting the latest achievements in solid state physics, sometimes with results that have not yet appeared in monographs. This relates both to experimental discoveries and theoretical ideas. There are articles on high-temperature superconductivity, the quantum Hall effect, Kosterlitz– Thouless phase transitions in two-dimensional systems, autowave processes, fractals, etc. Novel nontraditional materials and techniques for investigation are described: amorphous substances, liquid crystals, quasi-crystals, polymers, low-dimensional systems, etc. In addition let us point out to the reader the “quantum-mechanical emphasis”, which may be noted in many articles devoted to diverse macroscopic phenomena and properties of solid bodies. Traditionally, use is made of the point of view that the quantum statistics of quasi-particles undoubtedly deﬁnes such macroscopic low-temperature properties of crystals as speciﬁc heat and thermal conductivity, electrical conductivity and magnetism. However, some authors only assign to quantum mechanics the role of describing microscopic laws explaining the dynamics of atomic particles. The discovery of high-temperature superconductivity transferred the quantum manifestations of particle dynamics into the region of moderately high temperatures. State-of-the-art experimental techniques make it possible to observe a number of phenomena involving macroscopic quantum tunneling. Thus, macroscopic solids fairly often exhibit some particular quantum features. Finally let us stress the role of models in solid state physics. As is well known, a model is a much simpliﬁed speculative scheme which allows a researcher, on the one hand, to propose a simple qualitative explanation of a property or phenomenon under study, and, on the other hand, to give a quantitative description of properties and to perform a complete theoretical calculation of characteristics of the phenomenon being studied. Models are utilized very often in solid state physics. Apparently, the most ancient model is that of an “absolutely solid body”. The model of perfect gas of quasi-particles is frequently employed; Ising’s model is well known in the study of magnetism. The model of a two-dimensional lattice of classical spins in the theory of phase transitions proposed by Onsager allowed him to give the ﬁrst statistical description of second-order phase transitions. The Frenkel–Kontorova and Peierls models are widely used in dislocation theory. References to them can be found in many of the articles included in this work. The need for this publication arises from the recent tremendous progress in this ﬁeld of physics, especially by the extension of its areas of practical applications. There have appeared new ﬁelds of electronics (optical electronics, acoustoelectronics); semiconductor electronics has changed and now employs an increasingly wider range of complex structures such as metal–insulator–semiconductor devices and computers with superconducting elements (cryotrons); and memory elements based on new physical principles have been developed. There are many promising new solid state materials based on garnets, rare-earth metals, magnetic semiconductors, amorphous metals, semiconductors, and, ﬁnally, the discovery of high-temperature superconductors in 1986. The compilers of this Dictionary hope that this publication will be useful for researchers working in solid state and other ﬁelds of physics (nuclear physics, plasma physics, etc.) and also for a wide audience of other readers, including, but not limited to, engineers investigating and utilizing solids, as well as doctoral and advanced students at universities. V.G. Bar’yakhtar A.M. Kosevich

HOW TO USE THE ENCYCLOPEDIC DICTIONARY In this Dictionary, we follow standard fundamental rules generally adhered to in encyclopedic publications. 1. Articles are arranged alphabetically; if a term (typeset in boldface) has a synonym, then the latter is given in the entry after the main meaning of the term (after comma, in usual print). 2. Some terms in the titles of articles adopted from other languages are followed by a brief etymological note (with clear abbreviations: abbr., abbreviated, fr., from; Gr., Greek; Lat., Latin; Fr., French; Germ., German, etc.). 3. The names of scientists appearing in the title or text of an article are commonly followed by the date of obtaining the result (effect, phenomenon) under consideration. 4. We use a system of cross-references (in Helvetica italics) to other articles. Additional terms explained within the same article are typeset in Times italic and, together with the main entries, are listed in the Subject Index at the end of Volume 2. Many terms synonymous to those in the article titles may be also found in this Subject Index. 5. Units of physical quantities and their symbols are given in the systems of units most commonly used in solid state physics. For the relations which convert these units into SI, see the tables included in the article Units of physical quantities. 6. The ﬁgures are explained either in their captions or in the text of the article. 7. Usually, the notation used in formulae is explained in the text of that article. However, some symbols have the same meaning throughout the Dictionary (unless otherwise speciﬁed): c, speed of light; h and = h/2π , Planck constant; T , absolute temperature; kB , Boltzmann constant; λ, wavelength; ν and ω = 2πν, frequency. The notation of some elementary particles is also standardized: ν, photon and gamma quantum; e, e− , electron; p, proton; n, neutron; d, deuteron; π and π ◦ , pions; μ± , muons; K ± and K ◦ , K-mesons.

xvii

This Page Intentionally Left Blank

Aa ABLATION (fr. Lat. ablatio, removal, taking away)

ABRIKOSOV–SUHL RESONANCE (A.A. Abrikosov, H. Suhl, 1965) The abnormal increase of the electron spin- ip scattering amplitude of conduction electrons on a

The removal of mass from the surface of a solid brought about by a heated gas ﬂow sweeping past it.

paramagnetic impurity when the energy ε of the scattered electron approaches the Fermi energy εF of the metal. The cause of the Abrikosov–Suhl resonance is the creation of a long-lived bound state of a conduction electron with a paramagnetic impurity due to the indirect interaction of conduction electrons with each other via the impurity spin when the spin–paramagnetic impurity exchange interaction constant is negative, i.e. J < 0. The Abrikosov– Suhl resonance manifests itself below the Kondo temperature T K by an anomalous temperature dependence of the behaviour of the resistivity and the magnetic susceptibility of a metal (see Kondo effect). The expression for the resistivity of a metal is derived by the selective summation of the “dangerous” terms of the perturbation expansion in the parameter |J |/εF 1 (diagrams calculated in the so-called parquet approximation), and has the form −2 εF J ν(εF ) (0) , ln ρ = ρs 1 + n kB T

This is observed during the motion of material bodies and space crafts through the atmosphere at high velocities. Ablation occurs as a result of erosion, melting, and sublimation. It is used to cool key parts of super- and hypersonic aircrafts, spacecrafts, and rocket engines by coating them with layers of an ablatable material (e.g., ceramics, or pyrolytic graphite). The ablation material must have high melting and sublimation temperatures and a large speci c heat.

ABRASIVE MATERIALS, abrasives (fr. Lat. abrasio, scraping)

Fine-grained solid materials intended for working (polishing, ﬁnishing) a material surface. The working consists in cutting and scraping the surface by a great number of randomly oriented sharp edges of abrasive grains. Typical abrasive materials are diamond (natural or synthetic), carborundum, the cubic modiﬁcation of boron nitride, and boron carbide. Abrasive materials are characterized by hardness, strength, granularity (describing the magnitude and dispersion of the grain size); knowing these parameters permits the selection of abrasive materials for particular purposes, and provides the expected precision of the working. Depending on their relative abrasive abilities, abrasive materials can be classiﬁed in terms of the following scale: diamond (1.00), cubic boron nitride (0.78), boron carbide (0.60), silicon carbide (0.50), and titanium carbide (0.42).

(0)

where ρs

is the resistivity calculated in the ﬁrst

Born approximation, ν(εF ) is the conduction density of electron states at the Fermi energy, and n is

the metal density. The denominator vanishes at the Kondo temperature εF n . exp − TK = kB |J |ν(εF ) In the temperature range T TK , perturbation theory is no longer valid, and a more detailed analysis shows that a spin complex of a conduction electron with an impurity is created, where at 1

2

ABRIKOSOV VORTICES

T = 0 the impurity spin is shielded by the conduction electrons. In the vicinity of TK the spin parts of the thermodynamic and kinetic characteristics of a metal sharply change their temperature dependences, remaining ﬁnite over the entire temperature range. The exact solution of the Kondo problem was obtained by P. Wiegmann and N. Andrei (1980). ABRIKOSOV VORTICES, vortex laments (A.A. Abrikosov, 1956) Vortex current structures of type II superconductors in magnetic ﬁelds with strength higher than the lower critical eld Bc1 (T ), but lower than the upper critical eld Bc2 (T ), i.e. in the domain of the mixed state (see also Shubnikov phase).

First predicted theoretically and then observed experimentally Abrikosov vortices are topologically stable singlet states, involving the penetration into a superconductor of minimal magnetic ﬂux quantities, equal to the ﬂux quantum Φ0 (see Quantization of ux). One can think of these vortices as quantum “rods” of magnetic ﬂux encircled by superconducting current ﬂow and pierced by magnetic ﬁeld lines (Fig. 1). For an isolated

Fig. 1. Abrikosov vortex. The arrows show the direction of the supercurrent ﬂow. The normal phase core region is cross hatched. The coherence length ξ and penetration depth λ are indicated.

Fig. 2. Behaviour of the order parameter Δ and the magnetic ﬁeld strength B in the region of an isolated vortex. Within the core (r < ξ ) the order parameter |Δ| decreases rapidly, reaching zero at the center.

Abrikosov vortex, the outer diameter has a radius equal to the London penetration depth λL (see Penetration depth of magnetic eld), and inside there is a core of radius equal to the coherence length ξ , in which superconductivity is suppressed by the high density of encircling shielding current that supports the magnetic ﬁeld (Fig. 2). One circuit around the vortex axis changes the phase of the order parameter Δ by 2π . The magnetic ﬁeld is able to penetrate the superconductor in the form of vortices because of the negative surface energy of the N–S boundary in a type II superconductor. When an externally applied magnetic ﬁeld B is present there is a gain in energy via the formation of a microscopic inhomogeneous region with a maximal surface. The extent of the splitting is determined by the ﬂux quantization condition, whereby the minimal domain size pierced by the magnetic ﬁeld has the value (Φ0 /B)1/2 . Since this minimal size cannot be smaller than ξ , it leads to the limitation that superconductivity is only possible for magnetic ﬁelds smaller than the value Bc2 = Φ0 /2πξ 2 (upper critical ﬁeld). In an ideal type II superconductor, Abrikosov vortices arrange themselves in a triangular lattice due to their mutual repulsion (see Vortex lattices in superconductors). When transport current ﬂows perpendicular to the magnetic ﬁeld direction Abrikosov vortices can drift in the direction perpendicular to J and B due to the Lorentz force J × B, which causes the appearance of electrical resistance in the superconductor (see Resistive state). For a resistanceless supercurrent to ﬂow in a superconduc-

ABSORPTION OF ELECTROMAGNETIC WAVES

tor (called a hard superconductor) the Abrikosov vortices should be held in position by pinning sites or defects of the crystal lattice (see Kosterlitz– Thouless transition, Vortex pinning). ABSOLUTE DIAMAGNETISM, ideal diamagnetism

The state of a superconductor in which a magnetic ﬁeld is completely excluded from its interior at a temperature below its critical temperature Tc . This occurs when the applied magnetic ﬁeld B is lower than the thermodynamic critical magnetic e ld Bc (T ) for a type I superconductor, and lower than the lower critical eld Bc1 (T ) of a type II superconductor (see Meissner effect). This implies that in the superconducting state the magnetic susceptibility χ attains its highest negative value χ = −1 in SI units (χ = −1/4π in Gaussian units). Absolute diamagnetism is caused by the persistent supercurrents which circulate in the outer surface layer of the material and shield the interior from the penetration of magnetic ﬂux (see Penetration depth of magnetic eld). This diamagnetism results in repulsion between a superconductor and a magnet, and the levitation of a magnet above a superconductor. Absolute diamagnetism is utilized in the manufacture of frictionless bearings, and the operation of trains levitated above their tracks. ABSORPTION (fr. Lat. absorptio, suck)

Absorption is the uptake or extraction of ingredients dissolved in or mixed with the bulk of a gas or liquid by another solid or liquid material called an absorbent. Absorption is one of the cases of sorption. In contrast to the surface process of adsorption, absorption occurs in the bulk of the absorbent. Absorption can be complicated by the chemical interaction of the absorbing substance with the absorbent (chemisorption). Absorption is used in industry to separate the components of a gas mixture by selective absorbents, possibly obtaining them in pure form by desorption with absorbents that can be reused afterwards. Examples are (1) the absorption of butadiene during the manufacturing of synthetic rubber; (2) removing gases from harmful admixtures (e.g., H2 S, SO2 , CO2 , CO); (3) obtaining a gas product such as sulphuric acid by absorption of SO3 ,

3

(4) the extraction of hydrocarbon gases (natural and synthetic) from their mixtures (e.g., propanes, butanes and pentanes). ABSORPTION COEFFICIENT, absorption factor, absorptance, absorptivity

The ratio of energy (particle) ﬂux, absorbed by a given sample, to the incident ﬂux. The term “absorption factor” is sometimes used in reference to an absorption index that is deﬁned as the natural logarithm of the reciprocal of the absorption factor. ABSORPTION EDGE See Intrinsic light absorption edge. ABSORPTION INDEX

A quantity α, which is the reciprocal of a distance, by which radiation ﬂux in a parallel beam is attenuated by the factor of 1/e as a result of its absorption by the material (cf. Absorption coef cient). It is introduced to characterize radiation intensity I = I0 e−αx which decays exponentially with the distance (see Beer–Lambert law). The value of the absorption index in crystals may depend on the direction of propagation, and the type of polarization of the radiation (see Dichroism of crystals, Pleochroism). ABSORPTION, LOW-FREQUENCY See Low-frequency enhanced magnetic resonance absorption. ABSORPTION, NONRESONANT See Nonresonance absorption. ABSORPTION OF ELECTROMAGNETIC WAVES in superconductors

The decrease in intensity of radiation, which is due to the partial transfer of radiation energy to the normal vibrations in the superconductor and, ﬁnally, to the crystal lattice. The rate of absorption of electromagnetic energy by a unit surface area of a superconductor is proportional to the active component of its surface impedance. At T = 0 the absence of this electromagnetic wave absorption exhibits a frequency threshold, i.e. it exists for ω Δ (where Δ is the energy gap), when an electromagnetic ﬁeld quantum possesses

4

ABSORPTION OF LIGHT

enough energy to break a Cooper pair. Measuring this threshold is one of the methods for determining Δ. In the mixed state of type II superconductors the absorption of electromagnetic waves is related to energy dissipation in the lattice of Abrikosov vortices and their viscous motion. In this case the measurement of electromagnetic absorption allows one to determine the magnetic ﬂux resistance and the so called pinning frequency. In electromagnetic ﬁelds of high amplitude nonlinear effects arise which are related to the probability of generating vortices by the wave ﬁeld, kinetic decoupling of Cooper pairs, and many-quantum absorption processes. ABSORPTION OF LIGHT See Light absorption. ABSORPTION OF SOUND See Sound absorption. ACCEPTOR

An impurity or structural defect with a local electronic level in the band gap of a semiconductor which can receive electrons from the valence band. An acceptor center is charged negatively if its local states are ﬁlled with electrons, and it is neutral if the states are empty. A predominance of acceptors over donors produces p-type conductivity (see Holes) with a temperature dependence determined by the height (typically 4π , the input

13

hypersound pulse splits into 2π -pulses. Acoustic self-induced transparency has been observed experimentally in dielectric and ferroelectric crystals, alloyed by paramagnetic ions of the iron group, satisfying the conditions of acoustic paramagnetic resonance at liquid helium temperatures. ACOUSTIC SOLID-STATE RESONATOR A device involving acoustic vibrations in a

mode close to that of a standing wave, viz. when the distance between the end plates of an acoustic resonator is an integral multiple of half-wave lengths. Typically, an acoustic resonator is made from a piezoelectric material (see Piezoelectricity), and the oscillations are excited by an electric ﬁeld. Piezoelectric acoustic resonators are electrical twopole and multipole elements with the impedance exhibiting resonant behavior near resonant frequencies. These resonators exhibit a high stability of the natural oscillation frequency, a longterm one of ∼10−6 –10−8 Hz, and a short-term one of 10−8 –10−10 Hz and higher. These are used to stabilize oscillator frequencies (of resonators), and form amplitude responses of ﬁlters (ﬁlter resonators). ACOUSTIC SPECTROMETER

An experimental installation for measuring sound absorption and sound velocity dispersion.

An acoustic spectrometer comprises the following basic components: a source of electromagnetic ultra-high frequency (UHF) oscillations, a component to pass on these oscillations to an acoustic wave transducer with a connection to the sample under study, a UHF section from the sample to the receiving end of the spectrometer, and a recording device. Acoustic spectrometers typically employ pulse and pulse-phase measurement techniques, those with continuous oscillations being less common. As a rule, the spectroscopic measurements determine the absorption and sound velocity dispersion as functions of external parameters such as magnetic ﬁeld, temperature, pressure, etc., at a ﬁxed UHF frequency. In pulse acoustic spectrometers, these quantities are the pulse amplitude and its traveling time through the sample under study, while in pulse-phase acoustic

14

ACOUSTIC SPECTROSCOPY

spectrometers the pulse that passes through the sample is compared to a signal coherent with it. The changes in amplitude and traveling time of the pulse through the sample are determined by beating the measured pulse with a reference signal. Pulse and pulse-phase acoustic spectrometers operate in both “transmission” and “reﬂection” modes. In the ﬁrst case, two acoustic wave transducers are placed on opposite sides of the sample, whereas in the second one, the same transducer is used for exciting and recording the acoustic oscillations. The pulse duration must be much less than its transit time through the sample. Continuous wave acoustic spectrometers operate in transmission only, and are used in measurements requiring low sensitivity to absorption factor variations. To increase the acoustic spectrometer response, use is made of low-frequency modulation of external parameters, with subsequent synchronous demodulation or digital accumulation of the signal. ACOUSTIC SPECTROSCOPY of solids

A collection of methods for investigating the resonant and oscillatory effects induced by the interaction of acoustic oscillations with different subsystems (electron, nuclear, spin, etc.) in a solid. Acoustic spectroscopy of normal metals. The acoustic spectroscopy of pure metals in external magnetic ﬁelds at low temperatures is the most diverse case since a large number of non-damping low-frequency collective waves can exist in metals. Owing to the cyclotron character of conduction electron motion and its interaction with acoustic waves in pure metals at low temperatures, the oscillating and resonant features of the sound absorption and the sound velocity dispersion depend on the external magnetic ﬁeld. If the conditions kl, Ωτ 1 are met (l, τ are the length and time of the mean free path of conduction electrons, k is the wave vector of the acoustic wave, and Ω is the electron cyclotron frequency), one can observe a magnetoacoustic effect whereby particular electrons most effectively interact with the sound, as indicated by the magnitude and direction of the constant magnetic ﬁeld relative to k, and by the value of parameter ωτ (ω is the frequency of the sound wave). Particular phenomena appear, such as giant quantum oscillations of sound absorption

and velocity dispersion, geometrical resonance, acoustic cyclotron resonance, Doppler-shifted cyclotron resonance, coupled acoustic and electromagnetic waves. These magnetoacoustic effects can provide extremum cross-sections, Fermi surface geometry, cyclotron masses, Fermi velocities and other energetic and kinetic parameters of conduction electrons (see also Electron–phonon interaction, Electromagnetic generation of sound, Acoustic wave ellipticity, Rotation of acoustic wave polarization plane). Acoustic spectroscopy is also an effective technique for studying an energy gap and its dependence on temperature and crystallographic direction. Acoustic spectroscopy of paramagnetic centers in insulator and semiconductor crystals is based on the application of hypersound waves for investigating the electron energy spectrum structure and the electron–phonon interaction of paramagnetic centers based on hypersound acoustic paramagnetic resonance (APR) spectroscopy. The resonant absorption of hypersound corresponding to APR in dielectric or semiconductor crystals containing paramagnetic centers is associated with induced transitions between the levels of the electron paramagnetic centers’ energy spectrum, and the APR line intensity (resonant absorption value) is proportional to the electron–phonon coupling of the center. That is why the APR characteristics such as the resonant magnetic eld and line width, as well as their dependence on the temperature, relative orientation of the magnetic ﬁeld and crystallographic directions, yield direct and accurate data on the positions of the ground and excited energy levels of the paramagnetic center, and its interaction with selected crystal lattice vibrations (electron–phonon interaction). Hypersound APR spectroscopy is an effective technique for studying the energy spectrum of non-Kramers centers with forbidden magnetic-dipole transitions and, especially, paramagnetic centers with orbital degeneracy in cubic crystal e lds, involving a strong electron–phonon–ion interaction. Acoustic spectroscopy of magnetically ordered crystals. These crystals exhibit elementary excitations of magnetization, such as magnons or spin waves. The magnetic subsystem energy is determined by the electric (exchange) and magnetic (dipole–dipole and spin–orbit) interactions

ACOUSTIC WAVE AMPLIFICATION

which depend on the distances between atoms. Magnons interact with phonons and undergo mutual scattering. This interaction is especially pronounced at crossings of magnon and phonon spectral branches in the region of magnetoacoustic resonance. In this case, coupled magnetoelastic waves having the amplitude equally dependent on the magnetization and elastic strain propagate in the crystal. Hypersound investigations of magnetoacoustic resonance, which underlie acoustic spectroscopy of magnetically ordered crystals, provide direct data on the structure of the magnon spectrum. One measures the resonant absorption value and the hypersound velocity change in a magnetic ﬁeld as a function of the temperature for several relative orientations of the external magnetic ﬁeld and the crystal. Acoustic spectroscopy is highly effective for the study of phase transitions in magnetically ordered crystals. ACOUSTIC SPIN ECHO

Coherent acoustic response of an electric or nuclear spin system in a paramagnetic crystal to the application of an acoustic or acousticoelectromagnetic pulse sequence during its resonant interaction with a spin system. Through the spin–phonon interaction (see Spin Hamiltonian), the acoustic pulse creates an inphase precession of dipole moments or quadrupole moments which, after the end of the pulse, become dephased in the time T2 under the inﬂuence of relaxation processes. If the excitation pulse length is less than T2 , the spin system dynamics is independent of the excitation ﬁeld amplitude at that given time, but it is determined by its value in the preceding period. Therefore, the application of the second pulse after the time τ < T2 causes the reversal of the dephasing process so that the initial phased state is recovered after the time interval 2τ (so-called phase memory effect). In materials with a strong spin–phonon interaction acoustic oscillations are generated (acoustic echo-response) at the moment of full phasing, in addition to the generation of electromagnetic ﬁeld pulses. Acoustic spin echo is the acoustic analogue of the magnetic resonance spin echo and photon echo. Acoustic spin echo enables one to measure the relaxation time and the spin–phonon interaction. Spin memory accounts for such nonlinear effects as acoustic selfinduced transparency and induction.

15

ACOUSTIC VIBRATIONS of crystal lattice

A type (branch, mode) of small oscillations of crystal atoms, when a displacement of the center of mass of a unit cell occurs; sometimes they are

called translational vibrations. The dispersion law (the dependence of the frequency ω on the wave vector k) of acoustic vibrations for small values of k is linear: ω = vph k, where vph is the phase velocity of the atomic displacement waves. It is an ordinary sound wave (hence the term “acoustic branch”), i.e. a matter density wave with frequency 0–1013 s−1 . At high frequencies, the dispersion law becomes nonlinear. In a three-dimensional crystal, there are always three branches of vibrations: with k directed along the symmetric direction in the crystal, one longitudinal and two transverse modes exist (the same as for an elastic-isotropic medium), the displacement vectors in transverse waves being mutually perpendicular. The quanta of vibrations are referred to as acoustic phonons. See also Crystal lattice dynamics and Phonons. ACOUSTIC WAVE AMPLIFICATION by current carrier drift

An effect which is the reverse of the electronic attenuation of acoustic waves. Ampliﬁcation of acoustic waves by charge carrier drift occurs in semiconductors and layered structures of the piezodielectric-semiconductor type when the drift velocity of free current carriers exceeds the phase velocity of the acoustic wave. For this ampliﬁcation to occur the acoustic waves must interact with free charge carriers. The strongest and most extensively studied interaction mechanisms are those involving the piezoelectric effect (see Piezoelectricity) and the strain potential. The piezoelectric interaction is dominant in piezosemiconductors at low frequencies ( v s , the electron absorption coefﬁcient becomes negative, and for l/λ 1 it is given (in cm−1 ) by K 2q ωτM (1 − vd /vs ) , 2 ω2 τ 2 (1 − vd /vs )2 + (1 + q 2 r 2 ) M D (1) where K is the electromechanical coupling constant for the given direction of wave propagation, τ M is the Maxwell relaxation time, r D is the Debye screening radius, ω is the wave frequency, and q = 2π/λ. Eq. (1) provides, for the most part, an adequate description of experiments on acoustic wave ampliﬁcation in piezosemiconductors which exhibit moderate electron mobility: CdS, CdSe, ZnO, GaAs, etc. (μ = 50–5500 cm2 ·V−1 ·s−1 ). The general nature of the relation between the electron absorption coefﬁcient and the drift velocity is shown in Fig. 2. Experimentally obtained electron ampliﬁcation coefﬁcients are of the order of tens and even hundreds of dB/cm. The nature of the interaction changes with increased frequency and with increased mean free path of the carriers. As the wavelength approaches the carrier mean free path the energy exchange between free carriers and the waves ceases to be dependent on collisions. In the case of a purely αe =

Fig. 1. Phase relationships between potential wave oscillations (solid lines) and electron concentration oscillations (dashed lines) for three successive times (a), (b) and (c).

at wavelength λ undergo a large number of collisions. Due to momentum relaxation, the motion of electrons with the wave is not inertia-free: as a result, the peak values of the electron concentration lag behind the potential minima, and the majority of grouped electrons become located at those positions of the charge pattern where the wave ﬁeld accelerates electrons in the wave propagation direction (see Fig. 1(a)). As this takes place, the energy of the wave is transferred to electrons, and the wave decays. The generation of a current carrier drift in the wave propagation direction in a semiconducting crystal brings about a change of the value of the absorption. Once the drift velocity v d equals the acoustic wave velocity v s , the concentration maxima coincide in space with the negative potential peaks, and the electron absorption discontinues because the wave no longer expends energy on inducing electron transport (Fig. 1(b)). When v d > v s , the peak values of electron concentration are ahead of the negative peaks of the potential (Fig. 1(c)). The electrons, which had been accelerated by the drift ﬁeld are now decelerated by the alternating wave ﬁeld. The energy, which is acquired by electrons from the electron drift genera-

Fig. 2. Dependence of the absorption coefﬁcient α on the ratio v d /v s of the electron drift velocity to the wave velocity for the two limits ql 1 (curve) and ql 1 (straight line). Note that for both limits at v d = v s the coefﬁcient α changes sign.

ACOUSTIC WAVE ELLIPTICITY

collisionless interaction (l/λ 1), the energy exchange with the wave involves only those carriers (e.g., electrons), which exhibit the projections vT x of the thermal velocity on the wave direction x close to the acoustic wave velocity (see Landau damping). The role played by the remaining electrons is limited to shielding the wave piezoelectric potential. In the process of energy exchange, the carriers characterized by vT x < v s gain energy from the wave, whereas those of vT x > v s give up energy to the wave. In the absence of drift, as well as at 0 < v d < v s (or under the conditions of back drift), most of the carriers belong to the former group (i.e. exhibit vT x < v s ), and hence the wave is attenuated. Under supersonic conditions favoring the drift of carriers (v d > v s ), the electron velocity distribution exhibits a distinguishing inversion, namely, the electrons that give up their energy to the wave exceed the number of those that gain energy, and hence the sound wave is ampliﬁed. The energy of the source of the drift ﬁeld is transferred to the waves, and the electron absorption coefﬁcient (in cm−1 ) changes sign at v d = v s : √ 2 K 2 q π(vs /vT )q 2 rD vd αe = 1 − . (2) 2 vs (1 + q 2 r 2 )2 D

The ampliﬁcation coefﬁcient is a linear function of the drift velocity. The collision-free mode of interaction is easily observed in semiconductors featuring a high electron mobility, e.g., in n-InSb, at liquid-nitrogen and liquid-helium temperatures at sound frequencies 200–500 MHz. As the frequency increases (10 GHz), the piezoelectric coupling mechanism gives way to the strain-potential mechanism, which occurs in all semiconductors, not only in piezoelectric ones. At high frequencies and low temperatures the electron de Broglie wavelength in certain semiconductors becomes comparable to the sound wavelength. In this case quantum effects are of considerable importance in the acousto-electronic interaction. These effects manifest themselves in certain features of the screening of the electric ﬁeld, and the attenuation and “shutdown” of acousto-electronic ampliﬁcation at q 2p, where p is the Fermi momentum or thermal momentum, depending on the electron statistics used. The effect of ampliﬁcation of acoustic waves by

17

charge carrier drift may be utilized in acoustoelectronic ampliﬁers, which are the solid-state analogues of travelling-wave tubes. These devices convert a signal into an acoustic form, amplify it, and then convert it back into electromagnetic oscillations. The advantages of acoustoelectronic ampliﬁers are low values of mass and overall dimensions. These devices, however, are not free from serious drawbacks, such as: high heat dissipation, high supply voltages, low efﬁciency, losses by energy conversion, high noise level, etc. Some of these disadvantages may be eliminated either fully or partially by application of ampliﬁers that operate by surface acoustic waves. The latter devices are based on laminated structures of a piezodielectric-semiconductor, the surface acoustic waves being initiated and propagated on the piezoelectric surface, which adjoins the semiconductor. The acousto-electronic interaction in laminated structures is induced by virtue of ac ﬁelds that penetrate from the piezoelectric into the semiconductor. Ampliﬁcation of acoustic waves by current carrier drift was ﬁrst observed by A.R. Hutson, J.H. McFee, and D.L. White (1961) in CdS crystals. ACOUSTIC WAVE CONICAL REFRACTION See Conical refraction of acoustic waves. ACOUSTIC WAVE ELLIPTICITY

Quantitative characteristic of an elliptically polarized acoustic wave. The magnitude (absolute value) of the acoustic wave ellipticity (ε) is the ratio of the semiminor to the semimajor axes of the ellipse along which an element of volume of the medium of a propagating sound wave moves. The sign of the ellipticity indicates the direction of the motion. The limiting cases of ellipticity, namely ε = +1 and ε = −1, correspond to clockwise and counterclockwise circular polarizations while ε = 0 corresponds to a linearly polarized wave. The acoustic wave ellipticity is always accompanied by a rotation of the acoustic wave polarization plane. The acoustic wave ellipticity may be either related to the internal structure of the medium, or be due to the interaction of the matter with a magnetic ﬁeld (see Acoustic analog of Faraday effect, Acoustic analog of Cotton–Mouton effect, Rotation of acoustic wave polarization plane).

18

ACOUSTIC WAVE FOCUSING

ACOUSTIC WAVE FOCUSING Concentration of the sound energy in a small region by the formation of a convergent wave front.

acoustic channels in space, and increasing the efﬁciency of the non-linear wave interaction.

In an isotropic medium the convergent wave fronts are portions of spherical and cylindrical surfaces. The minimum sizes of focused regions are of the order of the sonic wave length. Focusing is used for its local effect in small regions of space in the medium under investigation. Acoustic lenses and reﬂectors of corresponding shape may be used as focusing elements.

ACOUSTIC WAVE REFRACTION

ACOUSTIC WAVEGUIDE

A region of a medium relatively small in crosssection compared to its length, which localizes acoustic wave energy for the transmission and processing acoustic signals. The energy localization inside the wave-guiding structure is inﬂuenced by the acoustic nonuniformity of the medium. In the case of a smooth nonuniformity, the velocity proﬁle of an acoustic plane wave must have a minimum inside the structure in order to focus acoustic waves into the waveguide, taking into account wave front curvature. In the case of a sharp nonuniformity of the acoustical properties at the boundary, almost all the energy is localized inside the waveguide, and is retained there owing to the repeated reﬂections from the boundaries. The interference of the waves produces a complicated ﬁeld pattern in the waveguide arising from the superposition of normal modes of acoustic oscillations. Most widespread are planar acoustic waveguides which are inhomogeneous structures on the surface of substrates: strip waveguides formed from applied strips of another material, topographic waveguides involving grooves and ridges etched on the substrate, and diffusion waveguides wherein the inhomogeneities arise from the implantation of impurities in the substrate. There are also ﬁber acoustic waveguides. Distinctive features of the waveguide propagation are the presence of many acoustic vibration modes with strong dispersion. The latter is widely used for the development of dispersion devices for acoustic signal processing: ultrasonic delay lines, ﬁlters, waveguide lenses. The pronounced energy localization inside a waveguide enables the directing and transmitting of acoustic signals: without loss from the wave divergence, multiplexing

Variation of the direction of wave propagation in a nonuniform medium caused by the dependence of the phase velocity on the coordinates. The term “refraction of acoustic waves” refers to cases where geometrical acoustics is applicable, and it means the refraction of sonic beams at a planar or smoothly bent (on the scale of wavelengths) interface between two media. In the medium with a continuous dependence of the phase velocity on the coordinates the beam direction varies continuously, which involves refraction of waves. At the interface between two anisotropic media (see Bulk acoustic waves, Elastic modulus tensor) one incident plane harmonic elastic wave in the general case excites three waves – one quasi-longitudinal and two quasi-transverse refracted, and three reﬂected waves (see Re e ction of acoustic waves). The wave vectors of all these waves lie in the plane of incidence, determined by the normal to the interface and by the incident wave vector. In anisotropic cases refraction of the wave vector in the reﬂection of energy (sonic beam) from the interface can also occur (see Group velocity). ACOUSTIC WAVE ROTATION See Rotation of acoustic wave polarization plane. ACOUSTIC WAVE SCATTERING in solids

The process of formation of weak additional sound waves, differing in their characteristics from the incident wave, as a result of acoustic diffraction in a medium with inhomogeneities or obstacles. The process of scattering may be either coherent or incoherent, depending on whether the frequency of the vibrations is conserved or not during the scattering. In either case the scattering results in the attenuation of the sound wave. An example of incoherent acoustic wave scattering is the observation of hypersound in a dielectric crystal at low temperatures when the condition ωτ > 1 is satisﬁed (ω is the hypersound angular frequency, and τ is a thermal phonon lifetime). Absorption in that case is due to a three phonon scattering process whereby the incident phonon

ACOUSTO-ELECTRIC EFFECT

ﬂux forms a hypersonic wave of thermal phonons with long lifetimes, a result which arises from anharmonic vibrations of the crystal lattice. Irreversible absorption of the hypersound takes place, with the incident energy transferred to the thermal phonons. For coherent acoustic wave scattering off static inhomogeneities in a solid, scattered waves of the same frequency appear, with characteristics that depend on the type of incident wave, the inhomogeneities, and the boundary conditions at the surface. An example of such a coherent process may be found in the scattering of sound from crystalline inhomogeneities, such as the temperature-independent residual attenuation of hypersound in dielectric crystals at low temperatures. ACOUSTIC WAVE, SUBSURFACE See Subsurface volume acoustic waves. ACOUSTIC WAVE, SURFACE See Surface acoustic waves. ACOUSTIC WAVE TRANSDUCER

A device which transforms an electromagnetic vibration into acoustic ones, and vice versa. The majority of acoustic wave transducers are reciprocal, i.e. they may serve both as emitters and as receivers of acoustic vibrations. In ultrasonic and hypersonic investigations of bulk acoustic waves the most common transducers make use of the piezoelectric effect (see Piezoelectricity) or the phenomenon of magnetostriction. In resonance piezoelectric transducers, which have a thickness equal to an odd number of half wavelengths, monocrystalline quartz or lithium niobate (see Niobates) plates are used as operating elements at frequencies up to 1 GHz. Alternative materials are barium titanate, lithium tantalate, bismuth germanate, and piezoelectric ceramics. At frequencies in the UHF range the resonance acoustic wave transducers are applied at the samples under investigation, or at the sound wave guides in the form of thin lms of ZnO, CdS and other piezoelectric materials. The alternating electric ﬁeld is applied and recorded at the piezoelectric element either by the direct insertion of the latter into the electromagnetic circuit, or with the help of UHF

19

resonators or transmission lines. A thin magnetostriction transducer of acoustic waves is a magnetic lm applied at the end of the sample. The ﬁlm magnetized by an applied magnetic ﬁeld is deformed by the oscillating magnetic component of the UHF ﬁeld. Improved matching of the impedance of the acoustic wave transducer with the UHF guides and resonators may be achieved with the aid of piezoelectric transducers based on the depletion layers of piezosemiconductors, formed with many-layered and many-element constructions. For the excitation and recording of surface acoustic waves one may employ counter-pin transducers, in which the distribution of the electromagnetic ﬁeld and the corresponding deformation at the sound guide surface is pregiven or ﬁxed. These acoustic wave transducers are also used for excitation and recording of volume modes, spread at an angle to the surface at which the transducer is placed. This mode of exciting volume oscillations is used in dispersion delay lines when the effect of the sound velocity dispersion is reﬂected by the passage through different distances of vibrations with different wave lengths. For measurements of the absolute values of crystal lattice vibrations capacitance transducers have found their wide application, with their design in the shape of ﬂat plate capacitors, one plate of which is rigidly connected with the sample. See also Phonon generation, Electromagnetic generation of sound. ACOUSTO-ELECTRIC DOMAIN

A stationary or moving region of strong electric ﬁeld and an elevated intensity of acoustic noise which forms in semiconductors as a result of the ampliﬁcation of thermal crystal lattice vibrations by the electric current at a charge carrier drift velocity faster than that of the sound (see Acoustoelectric effect). ACOUSTO-ELECTRIC EFFECT

Establishment of a constant current or electromotive force caused by the transfer of momentum and energy from a traveling ultrasonic wave to conduction electrons (see Acousto-electronic interaction). The capture of electrons by the local electric ﬁelds arising in the conductor under the action

20

ACOUSTO-ELECTROMAGNETIC EFFECT

of an ultrasonic wave leads to their being carried along in the direction of the sound propagation, and an acousto-electromotive force arises along the sample. When the sample is introduced into a closed electric circuit an electric current begins to ﬂow through it. The current density is jA.E. = −2μΓ I /v (G. Weinreich, 1957), where Γ is the coefﬁcient of sound absorption by the conduction electrons, I is the ultrasonic wave intensity, v is the sound velocity, μ = eτ/m is the mobility, τ is the mean free path time. As seen from the expression for jA.E. , the sign of the acousto-electric current or acousto-electromotive force EA.E. = jA.E. σ (σ is the conductivity) depends on the sign of Γ , and can change depending on the ultrasonic wave propagation direction, its damping, or its ampliﬁcation. During the propagation of a surface acoustic wave a transverse acousto-electric effect is observable. When a transverse acousto-electric current directed into the sample bulk arises along with the longitudinal one; this is linked with the wave localization on the surface. See also Acoustomagnetoelectric phenomena, Surface acoustic wave. ACOUSTO-ELECTROMAGNETIC EFFECT

The appearance of a magnetic moment in a semiconductor crystal under application of a sufﬁciently strong electric ﬁeld causing the ampliﬁcation of acoustic noise (phonons). The generated ﬂux of acoustic energy results in the movement of charge carriers (see Acousto-electric effect), and in some cases the charges may not move along the electric ﬁeld direction (e.g., in an anisotropic crystal where the direction of maximal noise ampliﬁcation may not coincide with that of the applied electric ﬁeld). As a result, a circular electric current begins to ﬂow around the sample, and hence the appearance of a magnetic moment. Acoustic energy ﬂux injected into a sample from outside can induce a magnetic moment in the absence of the external electric ﬁeld (acoustomagnetic effect). The nonlinearity of charge carrier motion is related both to the anisotropy of crystals, and the acoustic energy ﬂux nonuniformity. This phenomenon is also observable in metals. The acoustomagnetic ﬁeld arises, in particular, during the propagation of surface acoustic waves. In this case

the acting force ﬁeld is always nonuniform because the oscillatory displacement of the particles decays into the bulk of the sample. ACOUSTO-ELECTRONIC AMPLIFIER See Acoustic wave ampli cation. ACOUSTO-ELECTRONIC INTERACTION (AEI)

Interaction of acoustic waves with charge carriers (conduction electrons and holes in metals, semimetals and semiconductors). In metals, due to the Pauli’s principle, the interaction with acoustic waves (sound) involves only electrons with energies close to Fermi energy EF . There are two main mechanisms of AEI: (1) the deformation mechanism involves a change in periodic potential of the crystal lattice and a local change of the dispersion law of quasi-particles E(p) in the electron Fermi liquid, (2) the electromagnetic mechanism is due to forces exerted on the electrons by electric and magnetic ﬁelds arising from the displacement of ions during the passage of the ultrasonic wave. For longitudinal sound, the ﬁelds are electrostatic and are screened by free electrons (see Electric charge screening) to a great extent. This leads to renormalization (p) of the strain potential Λik = λik (p) − λik (p), where the angle brackets indicate averaging the bare deformation potential λik over the Fermi surface. The quantity Λik can be interpreted as a distinctive phonon electric-charge in the metal. During propagation of the transverse sound wave the electrons are affected by the vortex electric ﬁelds (see Acousto-electric effect). In an external magnetic ﬁeld B, an additional, so-called induction interaction of the electrons with the acoustic waves arises, its strength being e(v · [U × B]), where v is the electron velocity, and U is the ion displacement velocity. This interaction involves the additional parameter (qRL )−1 , where q is the wave vector of the sound wave, and RL = pF /eB is the electron Larmor radius. The induction interaction prevails over the deformation in sufﬁciently strong magnetic ﬁelds when qRL < 1. Besides, in the presence of a magnetic ﬁeld AEI leads to various magnetoacoustic effects, in which electromagnetic resonances, ballistic and collective effects add their characteristic features.

ACOUSTO-ELECTRONICS

The great difference between the electron and ion masses leads to the fact that the sound velocity is many times less than the Fermi velocity of the electrons. This circumstance (adiabaticity) plays an important role in the interaction of electrons with sound. Adiabaticity supports introducing the concept of electrons and phonons as weakly interacting quasi-particles, and makes it possible to neglect inertial terms (Stewart–Tolman effect) in the AEI energy. In pure metals with a long mean free path l (ql 1) the adiabaticity underlies the fact that only electrons with a velocity v almost perpendicular to the sound wave vector can effectively interact with the sound (autophasing effect). In semiconductors, the AEI is mainly determined by the strain interaction related to the local change in the band gap under the action of the strain arising when a sound wave travels through the crystal. In ionic crystals and semiconductors with a large number of charged impurity atoms in the lattice, the electromagnetic mechanism of AEI is also possible. In superconductors, the AEI at temperatures lower than critical temperature of superconductors differs in some features from the AEI in normal metals. Due to the Cooper pairing of electrons (see Cooper pairs), the phonon absorption probability decreases and, as a consequence, a sharp (exponential) decrease of the ultrasound absorption factor occurs. Besides, the Meissner effect precludes the electromagnetic mechanism of AEI. ACOUSTO-ELECTRONICS

A branch of electronics dealing with the effects of excitation and propagation of acoustic waves in condensed media, the interaction of the waves with electromagnetic ﬁelds and electrons, and the development of acousto-electronic devices based on these effects. The diversity of effects utilized in the design of acousto-electronic devices suggests the division of acousto-electronics into the high frequency (microwave) acoustics of solids (effects of excitation, propagation and reception of high frequency acoustic waves and hypersonic waves), acousto-electronics proper (interaction of acoustic waves with conduction electrons in the bulk and on the surface of solids, see Acousto-electronic interaction), and acousto-optics (interactions between

21

light and acoustic waves). Acousto-electronics was formed as an independent part of electronics in the decade of the 1960s with the start of intensive studies stimulated by the discovery of the acoustic wave ampli cation by conduction electrons in cadmium sulﬁde crystals. The rapid development of acousto-electronics was caused by the necessity to create simple, reliable and smallscale radio signal processing devices for radioelectronic equipment. At the present time acoustoelectronic devices perform the following signal transformations: (1) in time (delaying and changing the duration of signals), (2) in phase and frequency (frequency and spectrum conversion, phase shift), (3) in amplitude (ampliﬁcation, modulation), and (4) those involving more complicated functional transformations (coding and decoding, signal convolution and correlation). In some cases, the acousto-electronic methods of signal transformation are simpler (as compared, e.g., to electronic methods) and, sometimes, they constitute the only possible choice. The use of these devices is predicated on the low propagation velocity of acoustic waves (compared to that of electromagnetic waves), weak absorption of acoustic waves in crystals with a high acoustic Q-factor (quality factor), as well as favorable interactions of these waves with electromagnetic ﬁelds and electrons. In acousto-electronic devices, both bulk acoustic waves and surface acoustic waves (SAW) are used. The manufacture of these devices employs piezoelectric materials and laminated structures composed of piezoelectric and semiconductor layers. Many acousto-electronic devices convert high frequency electric signals into acoustic waves (acoustic wave transducers) to propagate in a sound guide and then be converted back again into a high frequency signal. Components used for excitation and reception of bulk acoustic waves are mainly piezoelectric transducers: piezoelectric plates (at frequencies up to 100 MHz) and ﬁlm transducers (at frequencies above 300 MHz), while those employed for the excitation and reception of a SAW are opposite-pin transducers. The ultrasonic delay lines operating in the frequency range from several MHz to several tens of GHz, as well as quartz resonators for the radio frequency generator stabilization (see Acoustic solid-

0.10 no 2300 0.01 –

3138 3488 3295 3808 1681 2640 2505 3100 1010 2270 0.0017 0.045 0.05 0.014 0.015 0.015 0.073 0.09 0.062 0.01 ST, x y, z x, 112◦ x, 6.7◦ [110], [111] [110] z, 74.4◦ [100] [110], 24◦ –

state resonator), are among the most widely used acousto-electronics devices for bulk waves. The most common are acousto-electronic devices based on the SAW due to small loss for wave excitation, the possibility of wave propagation control at any point of a sound guide (along the wave propagation path), and the feasibility for designing devices with controllable frequency, phase and other responses. Such devices include resonators on the SAW, which are used as narrow-band acousto-electronic ﬁlters and are also introduced into a generator circuit for its frequency stabilization; delay lines (for long signal delay in memory elements); various ﬁlters based on the SAW (e.g., band ﬁlters, matched ﬁlters); coding and decoding devices and so on. The interaction of acoustic waves with conduction electrons in semiconductors and laminated structures of the piezoelectric–semiconductor type leads to such phenomena as electron absorption or ampliﬁcation of acoustic waves, the acoustoelectric effect, and others. These effects are useful in acousto-electronic generators. The nonlinear effects arising under the interaction of acoustic waves in piezoelectrics, semiconductors, and laminated structures of a piezoelectric-semiconductor type ﬁnd wide use in signal convolution and correlation devices. The interaction of light and acoustic waves in condensed media forms the basis for the operation of acousto-optic devices (deﬂectors, modulators, ﬁlters etc.). They can be used to control the amplitude, polarization, and spectral content of optical radiation, as well as its propagation direction (see Acousto-optics). ACOUSTO-ELECTRONICS MATERIALS

Pb[(Mn1/3 Sb2/3 )0.08 Zr0.42 Ti0.50 ]O3

α-quartz, SiO2 Lithium niobate, LiNbO3 Lithium tantalate, LiTaO3 Lithium tetraborate, Li2 B4 O7 Bi12 GeO20 Bi1.2 Sr0.8 TiSi2 O8 Pb2 KNb5 O15 K2.98 Li1.55 Nb5.11 O15 Tl3 VS4 Pb0.91 In0.03 [Zr0.44 Ti0.53 (Li3/5 W2/5 )0.08 ]O3

Coefﬁcient of electromechanical coupling Orientation Material (name, formula)

Table 1. Physical characteristics of some acousto-electronic materials

Speed of sound, m/s

Existence of cut with zero temperature coefﬁcient of delay yes no yes no no yes yes yes yes no

Acoustic loss in air (dB) at 100 MHz 0.03 0.04 0.03 0.04 0.0145 0.03 0.05 0.05 0.95 0.10

Industrial product Industrial product Industrial product Laboratory product Industrial product Laboratory product Specialized laboratory product Specialized laboratory product Specialized laboratory product Industrial product (high temperature and pressure) Industrial product (high tempetature and pressure)

ACOUSTO-ELECTRONICS MATERIALS

Comments

22

Materials used to create working parts for the branch of functional electronics, which involves devices and systems for processing large and extra-large (order of gigabits) information ﬂows. The physical basis for the operation of such devices is provided by the interaction of space and surface acoustic waves of various types (Rayleigh, Gulyaev–Bleustein, Love, etc.) with electromagnetic radiation ﬂuxes at various frequencies – from 10 to 1011 Hz. The main physical characteristics of some important acousto-electronics materials are given in Table 1. Some layered systems for devices are based on surface acoustic waves,

ACOUSTOMAGNETOELECTRIC PHENOMENA

23

Table 1. Physical characteristics of some layered acousto-electronic materials Material

Coefﬁcient of electro-mechanical coupling

Dielectric constant

Attenuation (dB) at 1 GHz

Carrier mobility, cm3 ·V−1 ·s−1

Ideal material Lithium niobate, LiNbO3 Bi12 GeO20 Lithium tetraborate, Li2 B4 O7 Quartz, SiO2 Aluminum nitride on colorless sapphire Zinc oxide on silicon Cadmium sulphide on silicon Gallium arsenide on silicon Silicon (substrate)

>0.010 0.045 0.013 0.012 0.012 (0.010)

3), all the states are localized provided the following inequality holds: t < γ W,

γ ≈ 1,

(1)

where t is the mean tunneling amplitude, or a quantity proportional to it, the width of the conduction band that would be created for W t . The value of γ is determined numerically. In the Lifshits model, the disorder is not speciﬁed by the spread in the site energies, but by the randomly positioned short-range impurities. In this model, Anderson localization takes place when the mean free path decreases to the order of the de Broglie wave length. If condition (1) for complete localization is not satisﬁed then the states in the central region of the band are not localized, but the ones

59

close to the top and bottom of the band still are. In this case, the electron system is in the insulating state if the Fermi energy EF is lower than the threshold energy (see Mobility edge) Ec ≈ W , and it is in the conducting state, if EF > Ec . The electrical conductivity behaves in the close vicinity of the metal–insulator transition point as follows: σ ∼ (t − γ W )ν σ ∼ (EF − Ec )ν ,

or ν = 0.5.

(2)

If the random potential in which the electrons move changes only slightly on a scale of the order of the electron wavelength, then the quantum value of the critical index ν = 0.5 “works” in a very narrow region, whereas in a wider region near the critical point the index ν takes on the quasiclassical value 1.7 predicted by percolation theory. All the preceeding remarks concern ordinary three-dimensional systems. It has been proven that in the one-dimensional case an electron has only localized states for any value of the disorder parameter W . Apparently this is also valid in the twodimensional case, except for the only inﬁnitely extended state in the middle of the band. Closely related to Anderson localization are such phenomena as weak localization and mesoscopics, in which the interference of electron scattering processes by several impurities, although weak, still plays a signiﬁcant role. It should be noted that Anderson localization is described in the single particle approximation. At ﬁnite temperatures, the inelastic particle interaction becomes signiﬁcant and cancels Anderson localization. However, it can be shown that selflocalization takes place even in an ideal crystal if inequality (1) is satisﬁed, where the quantity W has the sense of a characteristic level difference at neighboring sites. In an ideal crystal, this difference of levels is not due to impurities, but to the intrinsic interaction of particles with one another. Autolocalization has been observed in studies of the diffusion of 3 He atoms in solid 4 He. See also Elementary excitation spectra of disordered solids. ANDERSON MECHANISM OF HIGHTEMPERATURE SUPERCONDUCTIVITY (P.W. Anderson, 1987) A mechanism of superconductivity in systems

with “resonating” valence bonds (RVB).

60

ANDERSON MECHANISM OF HIGH-TEMPERATURE SUPERCONDUCTIVITY

This magnetic mechanism of Cooper pairing involves a fundamentally new type of ordering for two-dimensional systems with an antiferromagnetic Heisenberg interaction (see Antiferromagnetism). Proceeding from the experimental data on the insulating (La2 CuO4 ) and conducting (La2−x (Ba, Sr)x CuO4 ) phases of lanthanum compounds, Anderson proposed several hypotheses regarding their properties, and a possible superconductivity mechanism of high-temperature superconductors. The presence of bivalent copper Cu2+ with one hole in the unﬁlled 3d-shell classiﬁes La2 CuO4 as a magnetic insulator adequately described by Hubbard’s Hamiltonian (see Hubbard model) with a strong intra-atomic Coulomb repulsion hindering the free motion of the carriers (holes), and causing their localization (Mott metal–insulator transition). The Mott–Hubbard insulator ground state with one electron (hole) per atom (half-ﬁlled band) is equivalent to Heisenberg’s antiferromagnet (see Heisenberg magnet) with one spin S = 1/2 per site. A second Anderson suggestion based on H. Bethe’s works on one-dimensional magnetic materials, as well as on L. Pauling’s chemical bond theory, matches with the essentially quasi-two dimensional character of the structure of superconducting cuprates. The suggestion means that under certain conditions quantum ﬂuctuations, even at T = 0, are able to completely destroy antiferromagnetic ordering in the CuO2 planes, so that the complete wave function of the ground state of an individual plane can be represented by a linear combination of the wave functions of “valence-coupled” pairs of the localized carriers: C{n, m} (αn βm − βn αm ), ΨRVB = {n,m}

|ΨRVB |2 = 1,

n,m

(1)

where n, m are the bidimensional site vectors, {n, m} represent all possible conﬁgurations with contributions determined by the coefﬁcients C{n,m} , and αn , βn are functions of “up” and “down” spin projections. In this state, the mean value of a spin at each site is zero, but the phase coherence is retained. The lowest excitations above the ground state (1), known as spinons, are dangling bonds or individual unpaired spins. The lat-

ter are the topological defects (kinks), their thermodynamically equilibrium number being determined by the temperature. The kink displacement corresponds to the “valence bond transfer” from one site to another, with no change in energy and no transfer of charge taking place. It is in this sense that the state (1) corresponds to “resonating valence bonds”, while spinons (S = 1/2) turn out to be neutral, zero mass fermions. The transition from the insulating RVB-state to the metallic one is caused by introducing new holes into the system (by doping or a change in stoichiometry). The “extra” (free) holes are coupled to a spinon forming a new charged Boseparticle called a holon. The motion of holons both inside and between planes, their scattering by spinons, and the phenomenon of holon conﬁnement determine the ﬁnite resistance in the normal metallic phase, as well as the attraction with the formation of holon Cooper pairs, thereby facilitating a transition to the superconducting state at temperatures on the order of Heisenberg exchange interaction constant. The holon gas does not undergo a Bose–Einstein condensation. There is a relationship between the wave function (1) and the condensate wave function of the Bardeen– Cooper–Schrieffer theory

ΨBCS =

+ + a−k↓ |0, uk + vk ak↑ k

|ΨBCS |2 = 1,

(2)

+ where uk , vk are coefﬁcients, and akσ (σ =↑, ↓) are Fermi creation operators of carriers from the vacuum state |0. The wave function (2), projected on the pairs and then transformed into real coordinate space, acquires the functional form (1). Another feature of the Anderson mechanism lies in the possibility of a qualitative description of some unusual properties of high-temperature superconductors (such as the anomalous temperature dependence of the heat capacity, the resistance in the normal phase, anisotropy of conductance, etc.). Experiment shows that cuprate metal oxides in the normal state are ordinary Néel antiferromagnets. However, some arguments favor inducing the RVB-state in metal phases under conditions of strong spin interactions of free and localized carriers.

ANDREEV REFLECTION

ANDERSON MODEL (P.W. Anderson)

(1) In disordered systems theory – a strong coupling model with diagonal disorder described by Anderson’s Hamiltonian |nm| + εn |nm|, H =J n,m

n

where n, m are the sites of a d-dimensional lattice, n, m are pairs of the nearest neighbors, J is the transfer integral, and the energies εn at different sites n are independent, uniformly distributed random quantities. The pioneer work of Anderson gives arguments in favor of the fact that for d = 3, if εn are uniformly distributed in the interval [−W/2, W/2] and the quantity W/J exceeds some critical value (W/J )c , then all the states of this Hamiltonian are localized (Anderson localization). The Anderson model provides an effective analysis of the transition from quasi-Bloch (propagating) states to localized ones, and clariﬁes the presence and position of the mobility edge, characteristics of the ﬂuctuation elementary excitation spectra of disordered solids, and other properties of disordered solids. (2) In the theory of magnetism this approach provides a model Hamiltonian to describe the formation of the local magnetic moment of an impurity atom in a nonmagnetic metal as the impurity level changes relative to the Fermi level. The model admits an exact solution by means of the Bethe substitution (Bethe ansatz). (3) In the theory of metal-oxide superconductors – the model provides an explanation of resonating valence bonds (see High-temperature superconductivity, Anderson mechanism of hightemperature superconductivity). ANDERSON THEOREM (P.W. Anderson, 1959) A theorem stating that the electron scattering

by nonmagnetic impurities in superconductors has a slight effect on the critical temperature only. This theorem is based upon the invariance of the Hamiltonian with respect to time inversion. The Anderson theorem is not necessarily valid outside the framework of the Bardeen–Cooper–Schrieffer theory, namely, if one takes into account the weak localization of carriers, anisotropy of the Fermi surface, ﬁne structure of the density of electron states,

61

the presence of a dielectric gap on a part of the Fermi surface, etc. ANDREEV REFLECTION of quasi-particles (A.F. Andreev, 1964) A speciﬁc reﬂection of quasi-particles (electrons and holes) from the interface between the

superconducting (S) and normal (N) phases of a metal (NS-boundary).

During this process the quasi-momentum p of a reﬂected particle is conserved, but the signs of the charge and all three velocity components change. When an electron of energy ε (measured from the Fermi level) and velocity v = ∂ε/∂p is incident from the normal metal side on the NS interface, the reﬂected quasi-particle is a hole with the same energy ε and velocity v. The reﬂection of holes proceeds in a similar way. The value of the Andreev reﬂection coefﬁcient R depends on the quasi-particle’s energy: R(ε) = 1 for 0 < ε < Δ (Δ is the value of the energy gap in the superconducting phase); R(ε) → 0 for ε Δ. The essence of Andreev reﬂection is that at the NS-boundary the incident electron enters the superconducting condensate, forming a Cooper pair with an electron having the opposite momentum. A hole arising in the process moves back into the normal region. When the normal metal layer is situated between superconducting slabs (e.g., in the intermediate state of a superconductor or in SNS-junctions), Andreev reﬂection gives rise to distinctive quantization of the low-energy (ε < Δ) excitations of the N-layer (Andreev quantization). This quantization corresponds to a periodic motion of quasi-particles inside the N-layer, with the quasi-particle being an electron for half of the period and a hole for the other half. Andreev reﬂection manifests itself in a number of features of the thermodynamic and kinetic properties of the intermediate state of a superconductor. In particular, it leads to geometrical oscillation effects in ultrasonic attenuation, and to an additional thermal resistance of the intermediate state during thermal ﬂux propagation normal to N- and to S-layer, etc. As distinct from thermal ﬂux propagation, the passage of an electric current through the NS-boundary at low temperatures (kB T Δ) is not associated with overcoming the excess resistance of the S-boundary due to the quasi-particle

62

ANGULAR DEPENDENCE OF SPECTRA

reﬂection, since the conversion of the normal excitation current into that of Cooper pairs takes place under Andreev reﬂection. Andreev reﬂection has been directly observed experimentally in studies of the radio-frequency size effect, and of transverse magnetic focusing of electrons in NS-structures. ANGULAR DEPENDENCE OF SPECTRA of magnetic resonance The dependence of the resonant magnetic eld Br (in case of electron paramagnetic resonance, EPR) or resonance frequencies (in case of electron– nuclear double resonance, ENDOR; nuclear magnetic resonance, NMR) on the relative orientation

of the constant external magnetic ﬁeld B and the crystal axes, i.e. on the values of the polar angle θ and azimuthal angle ϕ that specify the B direction in a coordinate system relative to the crystal. The parameters of a generalized spin Hamiltonian are obtainable by comparing experimentally observed angular spectral dependences to those calculated from the Hamiltonian. Examining angular spectra in three mutually perpendicular planes permits determination of all parameters of the effective spin Hamiltonian (see Spin Hamiltonian para-

meters, Invariants), and the local symmetry groups of its interactions. An example of the angular dependences of the magnetic resonance spectra of the Gd3+ ion at a site of symmetry C2 is given in Fig. which plots the values of the resonant magnetic e ld Br versus the azimuthal and polar angles θ and ϕ, respectively, for the indicated transitions M → M − 1, where M is the eigenvalue of the projection of the electronic spin S = 7/2 on B. When the symmetry and arrangement of crystallographic axes (see Crystal symmetry) are unknown, they can be determined from EPR (NMR) spectra recorded for rotations around three mutually perpendicular axes ﬁxed in the crystal. In certain cases, the values of θ and ϕ also affect the line width and line intensity. An EPR spectrum is customarily called an anisotropic EPR spectrum, if the positions and intensities of its lines depend on the orientation of the sample relative to the external magnetic ﬁeld. For spin S 1 and in the absence of anisotropic hyper ne interactions, the anisotropic spectrum is observed only for centers belonging to non-cubic spin Hamiltonian symmetry groups, whereas in the presence of anisotropic hyperﬁne interactions

Angular dependence of EPR spectra of Gd3+ .

ANISOTROPIC MAGNETIC MATERIALS

with surrounding nuclei an anisotropic spectrum can be observed even for cubic symmetry groups. If the positions and intensities of EPR spectral lines are independent of the orientation of the sample under investigation relative to the direction of the external constant magnetic ﬁeld, then the spectrum is called an isotropic EPR spectrum. The concepts “anisotropic spectrum” and “isotropic spectrum” are valid also for other resonance phenomena such as NMR. ANGULAR MOMENTUM, moment of momentum

Vector product r × mv, where r is the position vector, v is the velocity of a material point of mass m. The angular momentum of an arbitrary system of points with masses mi , which move with velocities v i , is the sum of vector products

i r i × mv i , where r i is the position vector of the ith mass point relative to an origin of coordinates 0. The angular momentum depends on the choice of origin. ANHARMONICITY, VIBRONIC See Vibronic anharmonicity. ANHARMONIC VIBRATIONS of crystal lattices

Deviation from the simple harmonic nature of atomic vibrations in a crystal, i.e. a nonlinear relationship between the displacements of atoms (ions) from their equilibrium positions and the restoring forces. While the potential energy of a crystal in the harmonic approximation includes only terms of second order in the relative atom displacements, taking anharmonic vibrations into account leads to the appearance of cubic and higher order terms in the potential energy expansion in powers of the displacements. Anharmonicity of vibrations involves interaction between the normal modes (see Normal vibrations) of a harmonic crystal, which corresponds to taking into account both elastic and inelastic phonon collisions from the quantum point of view. Anharmonic vibrations are responsible for the thermal conductivity of insulators, the thermal expansion of bodies, the change in the dielectric function of the crystal with temperature, IR absorption and Raman scattering, etc. The anharmonic interaction of phonons leads to their scattering and decay which, in turn, determines the width (lifetime) and shift of the energy

63

levels. Accounting for the anharmonicity is a typical many-body problem, with its solution providing the answers to some fundamental questions of solid state physics, such as the possibility of forming two-phonon coupled states (biphonons), the role of soft modes in structural phase transitions, etc. Slightly and highly anharmonic crystals can be distinguished. Quantum crystals, systems with structural phase transitions, in particular ferroelectrics, fall into the latter type. The presence of solitons, which can contribute to the energy transfer and to the process of the restoring the equilibrium state after an external perturbation, is possible in an anharmonic crystal. ANISOTROMETER See Magnetic anisotrometer. ANISOTROPIC MAGNETIC MATERIALS Magnetic materials having different magnetic

properties along different directions. The most common anisotropic magnetic materials have one easy magnetization axis. Along this axis, high magnetization and low values of the coercive force are observed in soft magnetic materials and the maximal remanence is realized in hard magnetic materials. The magnetic anisotropy is natural for monocrystalline magnetics. The widely used polycrystalline anisotropic magnetic materials are obtained by a variety of methods. One of them is the production of crystallographic texture, i.e. preferable orientation of easy magnetization axes of individual crystallites along one common direction. Thus, in sheets of anisotropic electrical steel, the crystalline structure is produced by cold rolling and annealing, and in magnetically hard materials it is obtained by powder metallurgy which involves pressing in a magnetic ﬁeld. Another method of obtaining anisotropic magnetic materials involves producing magnetic texture by means of thermomagnetic treatment or thermomechanical treatment. In some anisotropic magnetic materials, both the crystallographic and magnetic texture are used simultaneously. Thus, e.g., the best magnetic properties are realized after thermomagnetic treatment of alloys of the alnico type, in which the columnar crystallographic texture is produced by directed crystallization.

64

ANISOTROPIC MEDIUM

ANISOTROPIC MEDIUM

A medium with some properties that depend on the spatial directions in it. Anisotropic media necessarily possess longrange order, involving translational and/or orientational order (see Long-range and short-range order). The natural anisotropy of crystals is related to the symmetry of the ordered arrangement of atoms (molecules) in space, and is the more pronounced, the lower the crystal symmetry. Many mechanical (anisotropy of elasticity, plasticity, hardness, etc.), thermal (thermal expansion and others), electric (electrical conductivity, dielectric constant, etc.), magnetic (magnetic anisotropy), and optical (birefringence) properties of monocrystals are anisotropic. Only a few crystal properties (e.g., density and speci c heat) do not depend on direction (isotropy). Ordinary liquids, in the absence of external factors, are isotropic like gases, due to the absence of long-range order in the relative positions and orientations of the constituent molecules (or atoms). The anisotropy of liquid crystals is due to the asymmetry and the long-range correlation of relative molecular orientations. The quantum liquid 3 He exists in two antiferromagnetic modiﬁcations: a highly anisotropic A-phase with weak ferromagnetic properties (in which superﬂuid motion is not always possible in some directions) and a weakly anisotropic B-phase. The inhomogeneity of a body in its surface layer results in local anisotropy of physical properties. Some chemical characteristics of a medium can also be anisotropic, e.g., the oxygenation and etching rates. The anisotropic properties of a medium can be characterized by corresponding tensor coefﬁcients (susceptibilities). ANISOTROPY FACTOR of a cubic crystal

This factor H = 2c44 + c12 − c11 depends on the elastic constants cij (see Elastic moduli). For an isotropic medium, H = 0 (see Isotropy). The anisotropy elasticity ratio deﬁned by A = 2c44 /(c11 − c12 ) has the value A = 1 for an isotropic medium. The quantity A can be either less than or greater than unity. For example, A has the values 1.00 for W, 1.21 for Al, 2.36 for Fe, 3.21 for Cu, and 0.69 for Cr. H is measured in Pa, and A is dimensionless.

ANISOTROPY FIELD See Magnetic anisotropy. ANISOTROPY, GROWTH See Growth anisotropy. ANISOTROPY, MAGNETIC See Magnetic anisotropy. ANISOTROPY OF CRYSTALS

Dependence of the physical properties of crystals on the direction.

The anisotropy is caused by the periodic arrangement of atoms in a crystal, and is related to the crystal lattice symmetry (see Crystal symmetry). Physical properties are the same only in equivalent crystallographic directions. According to the Neumann principle (see Crystal physics), the symmetry of any physical property cannot be lower than the symmetry of the point group of the crystal, but can be higher than that. Physical properties of crystals are described by tensors of rank from zero to four. Examples of properties described by a zero-rank tensor (scalar) are density and speci c heat (they are isotropic for every crystal). A ﬁrst-rank tensor (vector) describes, for instance, the pyroelectric effect, while thermal conductivity, thermal expansion and magnetic susceptibility are described by tensors of rank two. Tensors of third rank describe the piezoelectric effect (see Piezoelectricity) and electrooptical effect; most elastic properties of a crystal are described by a tensor of rank four. The symmetry of these properties depends on the crystal lattice symmetry. For crystals of low symmetry (triclinic, monoclinic), all these properties are anisotropic. Some of these properties for high symmetry crystals are isotropic, e.g., in a cubic crystal, all the properties described by a tensor of rank two are isotropic. ANISOTROPY OF ELASTICITY

Dependence of the elastic properties of a material on the spatial direction in it. The anisotropy of elasticity is characterized by the symmetry of its elastic modulus tensor, and by the values of its components. The elastic modulus tensor for an isotropic medium has the form Ciklm = λδik δlm + μ(δil δkm + δim δkl ), i, k, l, m = x, y, z,

(1)

ANISOTROPY OF LIQUID CRYSTALS

where λ and μ are Lamé coef cients. Any deviation of a tensor Ciklm from the form (1) corresponds to the presence of anisotropy of elasticity. In Voigt notation, the tensor Ciklm is replaced by the matrix cI J (I, J = 1, 2, . . . , 6) which, for the lowest symmetry, has 21 independent elements. The symmetry of interatomic interactions in a crystal imposes restrictions on the number of independent elements of cI J . If central forces act between atoms and every site of a crystal lattice is a center of symmetry, six Cauchy relations are satisﬁed: c12 = c66 ; c13 = c55 ; c23 = c44 ; c14 = c56 ; c25 = c46 ; c36 = c45 , which, for instance, in crystals with a heteropolar bond reduce to one relation: c12 = c44 . In hexagonal close-packed crystals no site is a center of symmetry, and the Cauchy relations do not hold even if the interatomic forces are central. The deviations from the Cauchy relations give an insight into the contribution of anharmonicity to cI J , and about nonpairwise (manyparticle) forces of interaction. Noncentrality of the interaction has a strong effect on the temperature dependence cI J = cI J (T ), as well as on the value cI I . The elements of cI J must satisfy a number of relations which are corollaries of the mechanical stability conditions for a crystal. For example, in a hexagonal close-packed crystal cI I > 0 (I = 1, . . . , 6); 2 − c2 > 0; c11 12 2 > 0; c33 (c11 + c12 ) − 2c13 2 > 0. c11 c33 − c13

Cubic crystals exhibit anisotropy of shift, which can be characterized by the factor Ashift = 2c44 / (c11 − c12 ). In addition to the shift anisotropy with the factor Ashift = c44 /c66 , crystals of hexagonal, trigonal and tetragonal symmetry have also an anisotropy of linear compressibility (with the factor Acompr = (c11 + c12 − 2c13 )/(c33 − c13 ) for hexagonal symmetry). Near the polymorphic transformation temperature, some combinations of elasticity constants can diminish abnormally (softening of normal modes). The defects in a crystal cause the components of the tensor of effective elastic moduli to decrease by several percent. When studying crystal distortions localized near defects, one needs to know elastic moduli tensors

65

of higher orders. The effective elastic moduli in a polycrystalline material are found by averaging over orientations of grains. ANISOTROPY OF g -FACTOR

A property which reﬂects the dependence of the splitting of electronic (nuclear) energy levels in a magnetic ﬁeld (see Landé g -factor) on the mutual orientation of the crystal and the ﬁeld. It manifests itself in the angular dependences of spectra of magnetic resonance, and is described by the second-rank g-factor tensor gpq (p, q = x, y, z) with unequal principal values. The magnitude of the tensor in the principal axis system for the po2 sin2 ϕ + lar angles θ, ϕ is given by g = [(gxx 2 2 2 2 2 1/2 gyy cos ϕ) sin θ + gzz cos θ] . For axial sym2 sin2 θ +g 2 cos2 θ)1/2 , where g = metry g = (g⊥ ⊥ gxx = gyy and g = gzz . Anisotropy is present in paramagnetic centers with a local symmetry lower than cubic. Ordinarily the tensor is symmetric, with gpq = gqp . ANISOTROPY OF LIQUID CRYSTALS

Dependence of physical properties of liquid crystals on the direction of a measurement.

In oriented samples the direction of the orientational order is speciﬁed by the director. If n , χ , and ε are respectively the refractive index, diamagnetic susceptibility and dielectric constant along the director, and n⊥ , χ⊥ and ε⊥ are the same quantities in a transverse direction, then

n = n − n⊥ , χa = χ − χ⊥ and εa = ε − ε⊥ are referred to as optical anisotropy, diamagnetic anisotropy and dielectric anisotropy, respectively. For example, for thermotropic liquid crystals n ∼ 0.1–0.4; χa ∼ 10−7 emu, εa ∼ 5–30. The sign of the anisotropy depends on the chemical structure of liquid crystals. For nematics (see Nematic liquid crystal), χa > 0, n > 0, εa > 0 and εa < 0. For cholesterics (see Cholesteric liquid crystal), χa > 0 and χa < 0, n < 0, εa > 0 and εa < 0. For smectics (see Smectic liquid crystal), χa > 0, n > 0, εa > 0 and εa < 0. Typical values for lyotropic liquid crystals are: χa ∼ 10−8 emu, n ∼ 10−3 . For lyotropic discotics χa > 0 and χa < 0, n > 0, for lyotropic calamitics χa > 0 and χa < 0, n < 0. Because of the anisotropy, the description of elasticity and viscosity of liquid crystals requires using several coefﬁcients.

66

ANISOTROPY OF MECHANICAL PROPERTIES

ANISOTROPY OF MECHANICAL PROPERTIES Differences in mechanical characteristics: elasticity, plasticity, and durability, along various direc-

tions of a solid. There are two types of anisotropy of mechanical properties: the natural or fundamental (primary) anisotropy, and the induced (secondary) type. The former is determined by the crystal symmetry (see Anisotropy of crystals) and can be easily observed. The latter is acquired during the process of mechanical and thermal treatment of a metal. There are two origins of secondary anisotropy: textural (see Texture) and structural. The textural type arises as a result of reorientation of crystallites along preferred crystallographic directions. The structural secondary anisotropy is caused by the oriented arrangement of grains and subgrains, inclusions of the second phase, and pores (see also Structural texture of metals). The elastic anisotropy for a number of textures can be derived analytically (see Anisotropy of elasticity). Anisotropy of plasticity and anisotropy of durability have more involved dependences than the anisotropy of elasticity, and are determined experimentally in mechanical tests. ANISOTROPY, OPTICAL See Optical anisotropy. ANNEALING Heat treatment of materials at elevated tem-

peratures aimed at investigating or improving their properties. Material annealing can lead to phase transitions, recrystallization, polygonization, homogenization, relaxation of internal stresses, removal of aftereffects of cold plastic deformation (strain hardening), annihilation and rearrangement of defects, and so on. The results of annealing depend signiﬁcantly on its kinetics: the rates of heating and cooling and the time of exposure at a given temperature. To investigate annealing of radiation-induced and other defects, use is made of isothermal annealing (long time exposure at constant temperature), and isochronal annealing (exposure during a given time interval at successively increasing temperatures). Various stages of isochronal annealing correspond to the presence of defects of different kinds. The annealing of the de-

fects of a particular type can lead to either their annihilation or their transformation into defects of more complicated types. The kinetics of isothermal annealing yield information on the nature of the reactions that result in the annealing. ANNEALING, IRRADIATION

See Irradiation annealing. ANNEALING OF SEMICONDUCTOR

See Pulsed annealing of semiconductors. ANNEALING, RECRYSTALLIZATION

See Recrystallization annealing. ANNIHILATION OF DISLOCATIONS

Merger and mutual destruction of two dislocations or elements of one dislocation loop with opposite signs (see Dislocation sign). The annihilation of dislocations leads to the disappearance (mutual compensation) of elastic e lds of dislocations. If parts of a dislocation with opposite signs come closer together as a result of dislocation slip in one common plane, then annihilation restores the perfect crystalline structure at their meeting point (see Fig. 1). The annihilation of screw dislocations occurs with the restoration of the structure even when they initially were not in the same slip plane. Nonscrew dislocations of opposite signs lying in different, but not too widely separated, slip planes form a dipole due to their mutual attraction. Its subsequent annihilation is possible by means of a head-on encounter with the creation of interstitial atoms or vacancies

Fig. 1. Annihilation of edge dislocations of opposite signs, which move in the same slip plane: (a) approach of the dislocations; (b) restoration of the perfect crystal structure upon annihilation.

ANOMALOUS DIFFUSION

67

ANOMALOUS AVERAGES

Fig. 2. Annihilation of edge dislocations of opposite signs, which move in neighboring slip planes: (a, c) approach of the dislocations; (b) formation of vacancy at the location of annihilation; (d) formation of interstitial atom at the location of annihilation.

(Fig. 2). When dislocations of opposite signs in different slip planes approach each other and reach a characteristic distance ra referred to as the annihilation radius, then the region of the crystal between them loses its stability, and annihilation occurs dynamically, rather then by diffusion. Studies of the dislocation annihilation process on an atomic scale by mathematical modeling provide the value ra ≈ (5–10)b, where b is the Burgers vector. The annihilation of dislocations plays an important role as an effective channel for reducing the dislocation density (see Dislocation density tensor) during the annealing process. This annihilation is accompanied by the emission of sound, and it is one of the most important mechanisms of acoustic emission.

The values of products of two (or more) cre+ (or annihilation akσ ) operators of halfation akσ integer spin particles (fermions), averaged over the lowest level (ground) quantum-mechanical states (at absolute zero temperature T = 0), or the thermodynamic states (at T = 0) of a system. The anomalous averages were introduced by N.N. Bogolyubov (1958) to describe superconducting (superﬂuid) Fermi systems in the self-consistent eld approximation. They provide the complex-valued order parameter (wave function) of a macroscopic coherent quantum state (see Macroscopic quantum coherence). In a superconductor at a temperature below T c , + + a−k−σ and the anomalous averages of the akσ a−k−σ akσ types are nonzero. They describe the condensate of Cooper pairs of electrons with antiparallel momenta (k = −k) and spins (σ = −σ ), which is analogous to a Bose condensate. In the super uid phases of 3 He at temperatures below 1 K (T < 0.003 K) and under a pressure (p > 30 atm), the triplet pairing of 3 He atoms with parallel spins (σ = σ ) is possible along with the singlet Cooper pairing (σ = −σ ), when the + + a−kσ and akσ a−kσ anomalous averages akσ do not vanish. In anisotropic crystals with a degenerate electron spectrum ε(k) = −ε(k + Q) and ﬂattened, nested regions of the Fermi surface separated by the wave vector Q, a spatially nonuniform state can arise. This state results from electron–hole pairing or a structural Peierls instability, and has nonzero anomalous averages of the + + ak,±σ and ak,±σ ak−Q,σ which type ak+Q,σ describe charge density waves and spin density waves.

ANODIZATION, anode oxidation

ANOMALOUS DIFFUSION A diffusion process in which the time evolution

The creation of a layer of oxide on the surface of a metal at a positive potential during electrolysis. Anodization is used to change the color, durability, hardness, electrical conductivity, catalytic activity, and other properties of surfaces of various metals and alloys. There is a great variety of electrolytes, and either direct or alternating current can be used. Depending on this, one obtains either a thin (less than 1 μm), or a thick (tens to hundreds of μm) enamel-like coating.

of the concentrations of diffusing particles fails to follow the Fick law, occurring asymptotically faster or slower than in the normal case. As for any diffusion process, anomalous diffusion is associated with a random walk of particles. However, in contrast to an ordinary random walk, the mean square displacement of a particle in the time t exhibits the behavior r 2 (t) ∼ t ν , with ν = 1. The causes of anomalous behavior are associated with the disorder of the system where the

68

ANOMALOUS DISPERSION OF LIGHT

random walk occurs. For example, anomalous diffusion behavior is observed in systems with a distribution of activation energies, when the distribution of the wait time of the next jump becomes very broad and the mean value of this time diverges; in a random walk in fractal systems the diffusion is slower (ν < 1); in a random walk with ﬂights, when a particle can travel a great distance during a short time (ν > 1), etc. To characterize anomalous diffusion, one often does not use the power index ν, but rather a related quantity called an anomalous diffusion index that characterizes properties of diffusion and random walk in a fractal system. In the normal case, for instance, on any Euclidean lattice, the square of the recession of a particle in random walk for sufﬁciently long time t is proportional to this time: L2 (t) ∼ t . In contrast to such universal behavior, the diffusion in a fractal system occurs more slowly, L2 (t) ∝ t 2/(2+θ) , where θ > 0 is the anomalous diffusion index. The quantity θ for fractal lines is related to the fractal dimension of the line D: θ = 2D − 2, although in other cases the quantity θ is some independent characteristic of a fractal system. The index θ for an inﬁnite cluster at the percolation threshold is related to well-known critical indices of percolation theory θ = (τ − β)/ν, where τ is the critical index of the percolation system conductivity, β is the critical index of the extent of the inﬁnite cluster, and ν is the critical index of the correlation length (see Correlation length). ANOMALOUS DISPERSION OF LIGHT Dispersion of light characterized by the anomalous dependence of the refractive index n of a ma-

terial on the frequency ν (wavelength λ) of the light: n decreases as ν grows (λ decreases). The anomalous dispersion of light occurs in the absorbtion bands of materials. ANOMALOUS ELASTICITY See Superelasticity. ANOMALOUS MAGNETORESISTANCE

The dependence of a conductor resistivity on the external magnetic ﬁeld, which is not describable within the classical picture of electron orbit bending (see Galvanomagnetic effects, Magnetoresistance). In magnetic materials: ferromagnetic and antiferromagnetic metals, semimagnetic

semiconductors, such departures from classic dependences (both in sign and in characteristic ﬁeld values) are related to the inﬂuence of the magnetic ﬁeld on the spin subsystem. In the case of nonmagnetic conductors, the anomalous magnetoresistance is caused by quantum-interference corrections to the conductivity, their contribution being determined by the coherence length (phase memory time) of the carriers. Such corrections arise both at weak localization (causing negative magnetoresistance), and due to interference of Coulomb and impurity scattering when the magnetoresistance is positive. ANOMALOUS MASS TRANSFER Transfer of inherent and impurity atoms in crys-

tals at a rate several orders of magnitude greater than that of diffusion. It is observed during pulse exposure causing plastic deformation with a rate greater than 1 s−1 . It results from dynamic recovery of nonequilibrium point defects formed during the process of plastic deformation under forging, explosion, pulse heating (thermoplastic deformation), in a pulsed magnetic ﬁeld (due to the action of ponderomotive forces). The mechanism of anomalous mass transfer consists in the creation of interstitial atoms under the nonconservative motion of dislocation thresholds at screw dislocations with a velocity higher than the critical one. The interaction of the moving dislocations with interstitial atoms causes the drift of the latter. Hence, the anomalous mass transfer can be treated as diffusion of nonequilibrium interstitial atoms under the conditions of drift (in the presence of driving forces of transfer processes). The distribution of the concentration C of diffusing atoms is described by the equation (x − V t)2 C(x, t) = C0 (4πDt)−1/2 exp − 4Dt x +Vt V Vx erfc √ , − C0 exp 4D D 2 Dt where C0 is the concentration at the instant of time t = 0; D is the diffusion coef cient, and V is the drift velocity in the x direction. The temperature dependence of the anomalous mass transfer rate is weaker than that of the diffusion coefﬁcient, and cannot in general be described by a simple exponential over a wide temperature range. The critical rate of deformation is deﬁned by the nonlinear

ANOMALOUS PENETRATION

dependence of the yield limit on the deformation rate. Below the critical rate, the energy of external stresses causing the dislocation slip is insufﬁcient for the formation of interstitial atoms. Therefore, only dislocation thresholds that create vacancies move conservatively. At fast rates, both vacancies and interstitial atoms are created. The latter prevail at small dislocation densities, so anomalous mass transfer diminishes with the extent of the plastic deformation. It diminishes also when an elevated concentration of excess vacancies is created in a crystal before the pulse arrival. The rise of the speed of dislocation displacement due to the swift rise of the external stresses leads to the diminishing of the vacancy contribution to the anomalous mass transfer. The dynamic multiplication of dislocations is superimposed, and the dragging along of interstitial atoms by shock waves begins to play a signiﬁcant role in the anomalous mass transfer. This transfer is faster in metals with face-centered cubic and hexagonal close-packed lattices than it is in those with a body-centered cubic lattice. The effect of anomalous mass transfer acceleration is more pronounced for substitutional impurities than for interstitial ones. As a result of the anomalous mass transfer, nonequilibrium solid solutions can also be created from the component with low mutual solubility in the solid phase. Under the low-temperature deformation of crystals with ionic bonds, other mechanisms of anomalous mass transfer appear. Thus, rather small deformation of LiF crystals at liquid helium temperatures leads to helium penetration into the surface layer of a crystal due to the dragging along of helium atoms by the dislocation thresholds, and their motion along the dislocations. Indentation (see Microhardness) of MgO crystals leads to directed plastic deformation (without the creation and motion of dislocations due to those of crowdions) (see also Anomalous diffusion). Engineering applications of anomalous mass transfer are diverse. Thus, hot forging or rolling of ingots of alloys at a deformation rate greater than the critical one allows considerable acceleration of the homogenization of dendrite liquation. Percussion welding in the solid phase forms welded joints of heterogeneous metals during a time too short for the creation of intermetallic compounds responsible for the embrittlement of the weld. The effective hardening

69

of the surface layer of machine parts is achieved by means of electric spark alloying. Taking anomalous mass transfer regularities into account leads to improving the alloyed surface layer obtained by laser processing (see Laser technology). Anomalous mass transfer occurs also at shot-blasting or ultrasonic treatment of a metallic coating on the surface of products. The mechanical mixing of surface layers of contacting metals under shock loading known as mechanical diffusion does not fall into the category of anomalous mass transfer. ANOMALOUS PASSAGE OF X-RAYS, Borrmann effect (G. Borrmann, 1941) Propagation of X-rays in monocrystals along directions satisfying the Bragg law, when the ef-

fective (so-called interference) absorption coefﬁcient is considerably smaller than the photoelectric absorption coefﬁcient μ. This is observed in the case of Laue diffraction for sufﬁciently thick crystals at absorption levels μt 3–5 (t is the sample thickness). The anomalous passage of X-rays is the result of multiple scattering by atomic planes of a crystal, and the interference of the scattered waves, which leads to the creation of a total wave ﬁeld with a spatially modulated amplitude. If the antinodes of this ﬁeld lie to the side of atomic planes, it is absorbed very weakly (much more weakly than in ordinary interference). As a result, the X-rays can travel in crystals for relatively great distances (up to 1–10 mm). The anomalous passage was ﬁrst observed in perfect crystals; and has subsequently been seen in mildly distorted crystals. It occurs for the diffuse background as well, which leads to considerable, often asymmetric deformation of the diffuse scattering of X-rays proﬁle compared to the kinematic case (ampliﬁcation of central part of the proﬁle relative to its wings). See also Dynamic radiation scattering, Two-wave approximation. ANOMALOUS PENETRATION of the electromagnetic eld into a metal

This occurs in an external magnetic ﬁeld, and is caused by the speciﬁc dynamics of the conduction electrons. The effects of anomalous penetration are subdivided into two groups. The ﬁrst group, that of plasma or collective phenomena, comprises the aggregate of weakly decaying waves in the degenerate electron plasma of a metal (see Helicon,

70

ANOMALOUS PENETRATION OF ULTRASOUND

Magnetic plasma waves, Cyclotron waves, Quantum waves, Doppleron, etc.). The second group in-

cludes ballistic effects of anomalous penetration which are caused by a trajectory transfer of an electromagnetic wave from the skin depth layer δ into the bulk metal by numerous groups of electrons, involving individual motions of the charged particles and quasi-particles. Because of the skineffect, the most effective interaction of the electrons with the electromagnetic ﬁeld occurs for those electrons which move along the wavefront, i.e. parallel to the surface of the metal (so-called effective electrons). Electrons moving at large angles with the surface spend less time in the skin layer, and thus are less effective in gaining energy from the wave. In a magnetic ﬁeld the direction of the electon velocity changes periodically due to the cyclotron motion. Therefore, the most intense interaction with the electromagnetic wave occurs in the vicinity of points of electron trajectories where the velocity is parallel to the surface (so-called effective points). Due to the cyclotron motion the number of these points is inﬁnite, and under the anomalous skin-effect δ D (D is the characteristic length of a trajectory), some of these points are located outside the skin layer. Their existence is related to resonant excitation of the electron collective motion. When moving inside this layer the electron acquires a velocity increase

v and creates the current j = −e v, where e is the magnitude of the electronic charge. At the next effective point lying in the depth of a metal, the electron again moves parallel to the sample surface and reproduces the current increment j there. This is what constitutes anomalous penetration of the ballistic type: bursts of current and magnetic ﬁeld spaced by the distance D arise inside the metal. The various types of electron trajectories lead to different mechanisms of anomalous penetration. In a magnetic ﬁeld B parallel to a metal surface, due to the complicated structure of the Fermi surface, there exists anomalous penetration along the chain of (closed) electron trajectories with extremal diameters Dext (see de Haas–van Alphen effect). The chain of trajectories from the central section of the Fermi surface is created in a slightly tilted B. At a greater inclination of B there occurs a kind of focusing of effective electrons drifting into the interior of the metal. These electrons

provide bursts of anomalous penetration at depths that are multiples of the displacement along the normal to the sample surface, extremal over the cyclotron period. This mechanism of anomalous penetration is related to a sharp rise of the Fourier component of the conductivity due to Dopplershifted cyclotron resonance. The following effects arise from the drift type of anomalous penetration: focusing of electrons from the vicinity of the reference point of the Fermi surface, bursts on the helical paths of the Fermi surface boundary cross sections, trajectory transfer by effective electrons on an open Fermi surface, etc. Finally, in a magnetic ﬁeld perpendicular to the metal surface, the ballistic effects of anomalous penetration are associated with the magnetic focusing of drifting or ineffective, electrons, the so called Gantmakher– Kaner effect. The various phenomena of anomalous penetration of trajectories of weakly damped waves are closely interrelated, and can transform into each other when the frequency ω or the magnetic ﬁeld B is changed. The physical pattern of anomalous penetration depends on the nature of the reﬂection of electrons from the metal surface. The anomalous penetration of radio waves manifests itself experimentally as a radio-frequency size effect. It is used to investigate Fermi surface parameters, the temperature dependence and anisotropy of the mean free path, and mechanisms of surface electron scattering. ANOMALOUS PENETRATION OF ULTRASOUND into a metal

A signiﬁcant nonlocal phenomenon appearing at high frequencies ω, when the damping depth of a sound wave (calculated within the framework of a local theory), L ∼ = vF /ω, is smaller than the mean free path of the carriers, l = vF τ (the latter is the penetration depth of electron density oscillations caused by sound, and interacting with it in a conductor; see Anomalous skin-effect). Thus, the anomaly criterion is ωτ 1 for the asymptote of the acoustic ﬁeld u(x, t) in the bulk of a metal (x L), when it is a relatively weak but slowly damped quasi-wave (non-exponentially damped in the collision-free limit) propagating with the electron velocity vF . The appearance of electron-acoustic quasiwaves is associated with the degenerate statistics

ANOMALOUS PHOTOVOLTAIC EFFECT

of charge carriers in metals, i.e. with the presence in the electron spectrum of a Fermi velocity in every direction. Anomalous penetration of ultrasound occurs for an arbitrary electron dispersion law, and for any polarization of the sound. In the typical case of a convex Fermi surface and monochromatic longitudinal vibrations, we have ωx s2 u(x, t) ∼ ln−2 = Cu(0, t) vF0 ωx vF0 x iωx , − × exp vF0 l0 vF0 x . ω Here C is a numerical factor of the order of unity determined by the form of the electron spectrum, and the nature of their reﬂection from the metal boundary (x = 0); s is the sound velocity, and vF0 = (vx )max is the electron velocity at the reference point on the Fermi surface. The quasi-waves are generated also by other particular values of vx on the Fermi surface; the power law of asymptotic decay u(x) ∼ x −3/2 as l → ∞ is characteristic for an internal extremum of vx on a nonconvex Fermi surface. With respect to short (compared with τ ) acoustic pulses, the anomalous penetration of ultrasound is revealed in the formation of an acoustic signal “forerunner” by electrons. In the absence of a magnetic eld the quasi-wave precursor travels with the velocity vF0 . Hence, the observation of the anomalous penetration of ultrasound in the pulse mode could make it possible, by varying the geometry and width of samples, to measure directly both electron velocities and local values of their mean free paths over the entire Fermi surface of the metal under study. Observed in the magnetic ﬁeld B in the pulse mode is the ultrasound ﬁeld transfer by conduction electrons along the electron orbit chain (the analogue of bursts of the electromagnetic ﬁeld). Having effectively interacted with the ultrasonic ﬁeld in the region where vx = s, the fast electron carries away the information on the sound pulse to create its “image” at its path locations where vx = s again. As a result, the forerunners and afterrunners of the sound signal arise, the distance between them (in the absence of electron drift along x) being a multiple of the extremal diameter of an electron orbit. To identify the effect

71

unambiguously, the generating ultrasound pulse width must be much less than the Larmor diameter. Otherwise, the effect appears as oscillations of the sound speed as the magnetic ﬁeld changes. The shape of the forerunners repeats that of the generating pulse. The analogue of the anomalous penetration of ultrasound is the anomalous penetration of an alternating longitudinal (i.e. normal to the interface) electric ﬁeld. Though its main part decays exponentially into the metal for a distance that approximates a Debye radius, the nonuniformity of the electron density remains down to macroscopic depths ∼ = l. Owing to the deformation interaction of a nonequilibrium electron gas with the ionic lattice vibrations, this leads to a new (linear in the applied ﬁeld amplitude) mechanism of electronacoustic transformation, where efﬁciency grows as ωτ increases. Such an effect related to the anomalous penetration of ultrasound was ﬁrst observed in a tin single crystal at liquid helium temperatures. ANOMALOUS PHOTOCONDUCTIVITY Photoconductivity which is characterized by

unusual behavior, such as: independence of the photocurrent from the photoexcitation intensity over a wide range, marked dependence on the spectral content of the light, and long-term relaxation of the photoconductivity after extinction of the light. Anomalous photoconductivity was discovered and investigated in detail on layers of amorphous selenium treated in mercury vapors. It is explained by the existence of deep traps for mobile particles with small probabilities of both thermal excitation of electrons to the conduction band, and recombination with a free hole. The traps are assumed to be clusters containing about 103 atoms, and localized in a region near the surface of the sample. Anomalous photoconductivity is sometimes referred to as the phenomenon of current reduction under illumination, but in this case the term negative photoconductivity is more often used. ANOMALOUS PHOTOVOLTAIC EFFECT

Appearance of a voltage Vp during illumination of a sample by light of energy in excess of the band gap Eg .

72

ANOMALOUS SKIN-EFFECT

Under ordinary mechanisms of the photoelectromotive force: eVp Eg (see Photoelectric phenomena). Anomalous photovoltages are observed in semiconductor ﬁlms (e.g., CdTe), in lithium niobate crystals, selenites and other materials exhibiting unipolarity along some direction. The values of Vp in the anomalous photovoltaic effect can be as high as many kilovolts. This effect can occur either with the absence of a center of symmetry of the crystal lattice, or with a certain nonuniformity of the distribution of defects in the sample. In the ﬁrst case, the appearance of a photovoltage provides for the transfer of free current carriers in one of the directions along the unipolar axis during the process of photoexcitation (such a mechanism was discovered experimentally in lithium niobate crystals), or is responsible for the unipolar character of current carrier scattering by oriented dipoles created by lattice defects. In the second case, the cause of the anomalous photovoltaic effect can be the formation of interconnected microscopic sources of electromotive forces, e.g., semiconductor junctions. This mechanism has been used to explain the anomalous photovoltaic effect in semiconductor ﬁlms. ANOMALOUS SKIN-EFFECT

A variety of phenomena of electromagnetic ﬁeld damping in metals (and plasma) under the condition that the mean free path l of conduction electrons considerably exceeds the skin layer depth, δ. In contrast to the normal (classical) skineffect when l δ and electromagnetic absorption is determined by collisions of conduction electrons with scatterers, the mechanism of absorption in the anomalous skin-effect has the collisionfree character of Landau damping. The screening of the external wave by the conductor in this effect is caused by the sliding (so-called effective) electrons that move almost in parallel to the surface at angles on the order of δ/ l. The salient features of the anomalous skin-effect are the non-exponential decay of the amplitude of an electromagnetic wave deep inside the metal, independence of the skin layer depth δ on l (in the normal skin effect δ ∝ l −1/2 ), a different frequency dependence of the surface impedance Za ∝ ω2/3 (whereas Zn ∝ ω1/2 ) and the change of the relation between its real and imaginary parts. The

value of the impedance in the anomalous skineffect depends on the character of electron scattering at the surface: under diffuse reﬂection, and the impedance is 12.5% greater than under specular reﬂection. The anomalous skin-effect has been observed in pure monocrystals of metals at low (helium) temperatures in the frequency range from several to hundreds of GHz. It was discovered by H. London (1940) in tin. ANOMALOUS THERMAL EXPANSION

Excessive thermal expansion of the lattice surface (in the ﬁrst 1–2 monolayers), which takes place in semiconductors, metals and simple chemical compounds. For example, the ratio of the linear thermal expansion coefﬁcient (normal and tangential) of the surface to its bulk value for a Si crystal is approximately 8, for Ge: 4, for GaAs: 3, for NaF and LiF: 2, for W: 2–3. Anomalous thermal expansion was established by various methods: low-energy electron diffraction, scattering of H and D atoms, spin polarization of reﬂected lowenergy electrons. This expansion does not harm the crystal surface (for moderately high temperatures) due to the relaxation (compression) of the surface layers of the lattice, and the presence of monatomic steps and other defects on the crystal surface. For instance, under heating to 500 K the lattice parameter of bulk LiF will rise by 1.5%, while the increase on the surface is 3%. The extra expansion (1.5%) of the surface is compensated by surface relaxation or structural defects. ANOMALY, KOHN See Kohn anomaly. ANTHRACENE, C14 H10 (fr. Gr. ανϑρας , coal)

An aromatic conjugated, condensed three ring hydrocarbon with molecular weight 178.22. A crystal of anthracene (speciﬁc weight 1.25 g/cm3 ; T melting = 217.8 ◦ C; T boiling = 355 ◦ C) consists of anthracene molecules bonded by weak van der Waals forces; it is a typical representative of molecular crystals. Crystals of anthracene belong to the prismatic monoclinic sys5 ) and two moletem with space group P 21 /c (C2h cules per unit cell. The monoclinic axis b, the

ANTIFERROELECTRICITY

crystal symmetry axis, coincides with the middle axis of the refractive index ellipsoid. Crystals of anthracene can be produced by sublimation, as well as by crystallization from the melt (Bridgeman’s method), or from solution. Using monocrystal growth by sublimation one obtains thin (from a fraction to hundreds of microns) colorless foils, their blue uorescence being readily observable under ordinary illumination (quantum yield of ﬂuorescence close to unity). The plane of these foils contains the a and b axes of the crystal. Anthracene is easily soluble in hot benzene, poorly soluble in alcohol, ether, and is insoluble in water. It is crystallized from solution to form colorless prisms. Using the Bridgeman method, one can obtain large crystals with any developed plane. Crystals of anthracene begin to absorb light in the near ultraviolet region. The Davydov splitting of the 0–0 band of the ﬁrst electron transition is equal to 230 cm−1 . Under irradiation with ultraviolet light anthracene can be dimerized or oxidized to anthraquinone. A crystal of anthracene is an organic semiconductor, and it is the basis of several large groups of dyes. Many valuable natural substances are anthracene derivatives (alizarin, cochineal, chrysophanic acid, etc.). Anthracene lm s produced by spraying can be used as nonsilver carriers for information recording. ANTICORROSIVE COATINGS

Layers of material applied to metal parts for corrosion protection.

The protection is assured either by insulation of the construction metal from the corrosive environment, or due to the protective or inhibitory action of the coating upon the metal being protected. In terms of composition, anticorrosive coatings are classiﬁed into nonmetallic, metallic and composite; and in terms of their mode of action they can be insulating, protecting and inhibiting. Concerning their durability, coatings are protective (for a given service life) and preserving (temporary protection). Some important properties of the coatings are their chemical resistance, porosity (permeability), adhesion to the basic metal, and deformability. The tin, lead, copper, nickel, chrome, and titanium coatings are classiﬁed as corrosion resistive (insulating) metallic coatings, while zinc, cadmium, aluminum coatings on steel are protective types.

73

Concerning their mode of application metallic coatings are subdivided into electroplated, hotdip (of the melted metal) and metallized ones. The nomenclature of metallized coatings is quite diverse, and is differentiated by the deposition method (electric arc, gas-ﬂame, plasma, and gasthermal metallization). To create coatings or corrosion layers on the metal surface, one can also use electrolysis from melted salts, deposition from gas-vapor phase, and implantation of metal ions or noble gases. To improve the operating protective properties of the surface layer, use is often made of diffusive heating that provides for diffusion of coating components into the underlying metal. The greatest scope of application (about 70%) involves protective polymeric (and ﬁlm) lacquer paint coatings, protective fettle coatings, protective enamel and other inorganic nonmetallic coatings differing in their chemical composition, technology of application and range of use. Composite metal-polymer coatings, inhibited metallic and nonmetallic coatings that provide better reliability and protection duration have gained wide use as well. ANTIEMISSION MATERIALS Metals, alloys, chemical compounds exhibiting

low intensity of electron emission or its absence. The antiemission materials include gold, platinum, titanium, zirconium, carbon, carbides of tungsten and molybdenum, titanium silicides, and others. They are used for coating the working surfaces of instruments, as well as their nonoperational surfaces to suppress electron emission during their useful lifetime. ANTIFERROELECTRICITY (fr. Gr. αντ ι, against, and ferroelectricity)

A set of phenomena related to the appearance of ordered antiparallel electric dipole moments in the crystal lattice of antiferroelectric crystals. The spontaneous polarizations (see Ferroelectricity) of neighboring ionic chains or dipole groups of the same type are oriented in opposite directions, so the total polarization is zero. Phases having the free energy (see Thermodynamic potentials) close to that of pyroelectric and ferroelectric states are usually considered favorable for forming antiferroelectric phases, because the phase transitions to paraelectric and ferroelectric states are

74

ANTIFERROELECTRICS

possible from these phases under a change of temperature, application of electric ﬁeld, pressure, and substitutions for some lattice ions. The electric ﬁeld decreases the temperature of an antiferroelectric phase transition and increases the dielectric constant ε. There are antiferroelectric phases with their structure change explainable by condensation of several soft modes having wave vectors on the Brillouin zone boundary. The phase transition from the para- to the antiferromagnetic phase is accompanied by a change in the lattice superstructure, reduction of ε, spontaneous strain, changing the birefringence and quadrupole bond constant, elastic and electrooptical properties, etc. More than 60 antiferroelectric compounds are known with many different structures. Some of them have a displacive type phase transition (e.g., PbZrO3 , NaNbO3 , PbMg1/2 W1/2 O3 ), and others with the perovskite type structure undergo an order–disorder phase transition (also NH4 H2 PO4 , Cu(HCOO)2 ·4H2 O). There are incommensurate nonpolar phases which are antiferroelectric in the crystals NaNO2 , Rb2 ZnCl4 and others. Antiferroelectrics are used as electrooptic materials and as components of various solid solutions, which are the bases of capacitor, piezoelectric materials and electrostriction materials for optics, electronics, radio engineering, and so on. ANTIFERROELECTRICS Insulators with internal oppositely directed elec-

tric dipole moments due, for example, to rows of ions displaced in opposite senses. A transition from the high-temperature paraelectric phase to the low-temperature ordered, antiferroelectric state occurs via a structural phase transition, which is accompanied by a considerable anomaly in the dielectric constant. The transition temperature TC typically depends strongly on the applied electric ﬁeld, so antiferroelectricity can be induced by the application of a ﬁeld, as well as by lowering the temperature. Since the transition is typically a r storder phase transition, a jump-like change in the polarization P is observed as the ﬁeld E changes, and the dependence P (E) has the shape of a (possibly double) hysteresis loop (see Hysteresis). Typical antiferroelectrics are NH4 H2 PO4 (TC = 148 K), PbZrO3 (TC = 506 K), and NaNbO3 (TC = 627 K).

ANTIFERROMAGNET

A material with antiferromagnetic ordering of magnetic moments of atoms and ions (see Antiferromagnetism).

A substance becomes antiferromagnetic when cooled below its Néel point T N , and generally remains in this state down to T = 0 K. Elemental antiferromagnets are: solid oxygen (α-modiﬁcation) at T < 24 K; Mn (α-modiﬁcation) with T N = 100 K; Cr (T N = 310 K); a number of rareearth metals (with T N from 12.5 K for Ce to 230 K for Tb). Chromium has a sinusoidally modulated magnetic structure, and the heavy rare-earth metals also have complicated magnetic structures provided by neutron diffraction (see Magnetic neutron diffractometry). In the temperature range between T1 and T N (0 < T1 < T N ), they are antiferromagnetic, and below T1 they become ferromagnetic. Chlorides of Fe, Co and Ni were the ﬁrst known antiferromagnets, and by now thousands of them are known. The chemical formula includes at least one transition ion. Antiferromagnets include numerous simple and complex oxides of transition elements such as ferrite spinels, iron garnets, orthoferrites and orthochromites, as well as ﬂuorides, sulfates, carbonates, etc. There are a few antiferromagnetic organic compounds, as well as metallic alloys, in particular alloys of the iron and platinum groups. The temperature dependence of the speci c heat has a maximum at T N which is typical of a second-order phase transition. Noted among cubic antiferromagnets is the family of rare-earth ferrite garnets in which Fe is replaced by Al or Ga. Dysprosium-aluminum garnet Dy3 Al5 O12 is of special interest because it is an antiferromagnetic Ising magnet in which the anomalous behavior close to the triple critical point has been studied in detail. The detailed investigation of hydrous copper chloride (CuCl2 ·2H2 O) led to the discovery of antiferromagnetic resonance, magnetic phase transition – reversal of sublattices (spin-ﬂop transition) in a magnetic ﬁeld, and weak antiferromagnetism. Noted among uniaxial crystals with anisotropy of the easy-axis type is the group of ﬂuorides (MnF2 and others), which served to clarify optical absorption spectra and provided the discovery of exciton-magnetic excitations, two-magnon absorption, and Raman scattering of light by

ANTIFERROMAGNETIC DOMAIN

magnons. The optical absorption spectra were also investigated with binary ﬂuorides like KMnF3 , CsMnF3 . Brillouin scattering of light by magnons was observed in antiferromagnetic FeBO3 and CoCO3 . In uniaxial CoF2 the piezomagnetic effect was discovered (see Piezomagnetism), and in Cr2 O3 the magnetoelectric effect. In uniaxial crystals with anisotropy of the easy-plane type (α-Fe2 O3 , MnCO3 , CoCO3 , NiF2 ) the weak ferromagnetism due to the Dzialoshinskii interaction was discovered. Of special interest among substances with weak ferromagnetism are the orthoferrites (YFeO3 and others) where orientational phase transitions (the change of the antiferromagnetic ordering axis) are observed, and transparent FeBO3 with T N above room temperature which displays a magnetoelastic interaction. The strongest magnetoelastic interaction among antiferromagnets is observed in α-Fe2 O3 . This is the ﬁrst compound to exhibit a wide gap in the spin wave spectrum that equals E = γ (2B ME B E )1/2 and is caused by the effective ﬁeld of magnetoelastic anisotropy B ME (B E is the exchange ﬁeld) (see Magnetoacoustic resonance). Some antiferromagnets contain more than two magnetic sublattices. For example, uranium oxide (UO2 ) is a four-sublattice antiferromagnet characterized by three antiferromagnetism vectors that form an orthogonal vector triplet. There is a group of antiferromagnetic semiconductors (chalcogenides of Mn, Eu, Gd and Cr) with very strong magnetooptical effects. The low-dimensional antiferromagnets are of particular theoretical interest. The already mentioned Fe and Co ﬂuorides as well as some binary ﬂuorides BaCoF4 , Rb2 CoF4 are two-dimensional antiferromagnets. The well-known metal-oxide compounds displaying properties of high-temperature superconductivity (La2 CuO4 , YBa2 Cu3 O7−δ ) in their insulating phase are many-sublatticed quasi-two-dimensional antiferromagnets. Onedimensional antiferromagnets include KCuF3 , CuCl2 , RbNiCl3 and others. Especially strong interactions of electron and nuclear spin system oscillations were observed in KMnF3 , MnCO3 , and CsMnF3 . Anhydrous sulfates of copper and cobalt as well as CoF2 exhibit antiferromagnetic ordering induced by a magnetic ﬁeld at temperatures above T N due to the Dzialoshinskii interaction.

75

The values of T N of most antiferromagnets lie below room temperature. ANTIFERROMAGNETIC DOMAIN A region of an antiferromagnet with a constant value of the antiferromagnetism vector L =

M 1 − M 2 . The directions of L in different antiferromagnetic domains are different. Antiferromagnetic domains are separated by antiferromagnetic domain walls. It is not always true that the division of antiferromagnets into domains results in a decrease of the energy of the demagnetization elds. The appearance of these domains either in the intermediate state of magnets, or for antiferromagnets with a weak ferromagnetism, is thermodynamically favorable. In other cases, these are thermodynamically unfavorable. In addition in some cases, e.g., for domains with zero magnetization and differing in the sign of L (antiferromagnetic domains with 180◦ neighbors), states in different domains, within the macroscopic framework, are considered identical because they differ from one another only in the redesignation of the magnetic sublattices. This is a substantial distinction of the properties of antiferromagnetic domains in comparison to, e.g., those of ferromagnets with different directions of magnetization. The presence of antiferromagnetic domains in real antiferromagnets can be linked with the fact that a magnetic phase transition to an antiferromagnetic state due to nonuniformity can occur independently in various ﬁnite regions of a crystal. If these regions differ in the sign of L, then the spreading of the transition over the whole sample causes antiferromagnetic domains to appear. In addition, the division of antiferromagnets into domains can reduce the energy of elastic strain, or (at moderate temperatures, near the Néel point) become thermodynamically favorable due to the contribution of entropy to the free energy of the antiferromagnet. These domains signiﬁcantly affect such properties as the electrical conductivity of a metal antiferromagnet, and sound absorption in some antiferromagnets. The presence of antiferromagnetism hinders the observation of a series of effects sensitive to the sign of L, e.g., piezomagnetism. Antiferromagnetic domains of the non180◦ kind (so-called T-domains or twin domains) are accompanied by a distortion of the crystal lattice, thus providing a way to detect, for example, a

76

ANTIFERROMAGNETIC METALS

conversion of an antiferromagnet to a single domain state, and to study it by various methods. The observation of the 180◦ antiferromagnetic domains (S-domains, i.e. spin-rotation domains) was carried out by using the linear magneto-optic effect. Those domains, in which this effect is allowed by the symmetry in the external magnetic ﬁeld, possess optical properties dependent on the direction of L, which allows one to employ optical methods for magnetic domain characterization. ANTIFERROMAGNETIC METALS Solids with metallic conductivity exhibiting antiferromagnetism. They include a number of 3d-, 4f -, and 5f -metals, their alloys and some

of their compounds. When analyzing the physical mechanism responsible for antiferromagnetism in the metals, it is important to know to what extent the electrons responsible for the magnetic ordering (magnetic electrons) are localized. Accordingly, one can speak about band antiferromagnetism (see Band magnetism) and the antiferromagnetism of magnetic ions. In band antiferromagnets the magnetic electrons form a relatively wide, partially ﬁlled band with the exchange splitting ε ζ , where ζ is the chemical potential referenced to the bottom of a band. These materials are described in terms of a static spin density wave with a wave vector k that can be either commensurate or incommensurate with a reciprocal lattice period (see Incommensurate structures, Modulated magnetic structures). A strict theory exists solely for the case of weak band antiferromagnetism ( ε ζ ). An example is pure Cr with the Néel point T N = 312 K. Below this temperature, the magnetic moment per atom is μ = 0.59μB (μB is Bohr magneton), much less than that of an isolated Cr atom (μ = 3μB ). The spin density wave period is incommensurate with the reciprocal lattice period k = (2π/a)(1 − δ, 0, 0), where a is the lattice constant. At T = 118 K, δ = 0.049 and depends slightly on the temperature; at T = T N , δ = 0.037. Chromium alloys can exhibit both commensurate and incommensurate spin density waves, the origin of latter being determined by the speciﬁc nature of the Fermi surface, which includes congruent hole and electron octahedra whose component parts can be made coincident with themselves via

translation by a reciprocal lattice vector k. It is the triplet pairing of electrons (holes) of congruent parts that manifests itself as a spin density wave with wave vector k. The presence of congruent parts of Fermi surfaces leads to instability of the paramagnetic state with respect to the emergence of a spin density wave (spin density wave instability). Weak band antiferromagnets include compounds with metallic conduction CrB2 (T N = 85 K), VX, VX2 , V3 X4 , V5 X8 , where X ≡ S or Se (for VS T N = 1040 K, for V3 S4 T N = 9 K, for V3 Se4 T N = 16 K, for V5 S8 T N = 29 K, for V5 Se8 T N = 35 K). The weak band antiferromagnet MnSi possesses a helical structure (see Helicomagnet) with a long wavelength (180 Å) and hence it may be considered as a weak band antiferromagnet with an inhomogeneous ground state in the form of a helical spin density wave. The examples of strong band antiferromagnets are: α-Mn (T N = 95 K); γ -Mn (T N = 450 K), γ -Mn being metastable in the region of antiferromagnetism (it is stable only at T > 1352 K); γ -Fe (T N = 8 K; γ -Fe is stable in the range 910–1400 ◦ C). They all support commensurate spin density waves. Antiferromagnetism of magnetic ions takes place in rare-earth metals due to the smallness of the radius of 4f -shells whose electrons are responsible for the magnetic ordering (see Magnetism of rare-earth metals). Rare-earth metals are commonly classiﬁed into light (from Ce to Eu) and heavy (from Gd to Lu) ones. The light rare-earth metals (except Nd) at T N are antiferromagnets with a collinear structure. In the heavy rare-earth metals (except Gd, Yb, Lu) and in Nd, an antiferromagnet–ferromagnet transition is observed at a lower temperature T = T c < T N in addition to the paramagnet–antiferromagnet transition at T = T N . In the antiferromagnetic range T N –T c , magnetic moments of rare-earth metals create complicated modulated magnetic structures (helical, cycloidal, sinusoidal). The complicated magnetic structures arise also in alloys of rareearth metals with each other and with Y (a paramagnet in the pure state). The Néel temperatures of the light rare-earth metals are as follows: for Ce T N = 12.5 K; for Pr T N = 20 K; for Sm T N = 14.8 K; for Eu T N = 90 K; for Nd T N = 19 K with ferromagnetism observed below T c = 7.5 K.

ANTIFERROMAGNETISM

Intermediate type of antiferromagnetic metals. The magnetic order of a number of antiferromagnetic metals is determined by the presence of two factors: spin density wave instability (near congruent parts of Fermi surface) and localized magnetic moments (FeRh, Pt3 Fe, alloys: Cr–(Fe, rare-earth metal), Mn–rare-earth metal, Y doped with rareearth metal). Small additions of rare-earth metals to paramagnetic Y cause a helical antiferromagnetic structure to appear. In compounds FeRh, Pt3 Fe, one part of the Fermi surface exhibits spin density wave instability, while another forms local moments. Antiferromagnetic actinides: pure metallic curium (T N = 52 K) and several compounds with metallic conductivity: UP (130 K), UAs (182 K), USb (213 K), UBi (290 K) (T N given in parentheses). ANTIFERROMAGNETIC RESONANCE

The selective absorption by an antiferromagnet of electromagnetic wave energy with a frequency close to the natural frequencies of precession of magnetization vectors of magnetic sublattices; a variety of electron magnetic resonance. Antiferromagnetic resonance involves the excition of resonant coupled oscillations of magnetization vectors of magnetic sublattices of the antiferromagnet relative both to each other and to the direction of the applied magnetic ﬁeld B 0 (see Antiferromagnetism). The frequency of these oscillations is determined by the value of effective magnetic ﬁelds acting on magnetic moments of sublattices: B E , the effective ﬁeld of the exchange interaction of sublattices, B A the ﬁeld of magnetic anisotropy, and B 0 . The dependence of the resonance frequency ω on the effective magnetic ﬁeld in antiferromagnets is complicated, and depends on the crystal structure. When the external magnetic ﬁeld is applied parallel to the easy magnetization axis then two antiferromagnetic resonance frequencies lying in the range 10–100 GHz correspond to one value of B 0 . The study of antiferromagnetic resonance makes it possible to determine the value of effective magnetic ﬁelds in antiferromagnets.

77

ANTIFERROMAGNETISM

Magnetically ordered state of a crystalline material in which neighboring atomic magnetic moments are aligned antiparallel, and the total magnetic moment of a magnetic unit cell of the crystal equals zero (or a very small fraction of an atomic moment). Antiferromagnetism occurs at temperatures below the Néel point T N . More generally, antiferromagnetism refers to the set of physical properties associated with the antiferromagnetic state. The exchange interaction seeking to align the spins and hence the magnetic moments antiparallel to each other is responsible for the antiferromagnetism. The idea that the exchange interaction can cause antiferromagnetism was put forward by L. Néel (1932) and independently by L. Landau (1933), who, in addition, described theoretically the phase transition from the paramagnetic to the antiferromagnetic states. At T > T N , when the thermal energy (E = k B T ) exceeds the exchange energy (μB E , where μ is the atomic magnetic moment and B E is the exchange ﬁeld), the material exhibits paramagnetic behavior (see Paramagnetism). The temperature dependence of the magnetic susceptibility χ of such a material at T > T N follows the Curie–Weiss law χ = C/(T − θ) with a negative Weiss constant θ , and C is a constant. At T = T N , antiferromagnetism appears in a material. In most cases the phase transition at T N is a secondorder transition accompanied by the characteristic anomalies of magnetic susceptibility, speci c heat, thermal expansion coefﬁcient, elastic moduli, etc. The magnetic ordering is characteristic of an atomic magnetic structure with a symmetry described by point and space magnetic symmetry groups. The magnetic structure of an antiferromagnet is conveniently described by two, four, or more interpenetrating magnetic sublattices with magnetizations M j that mutually compensate each other. As an example, Fig. 1 shows two antiferromagnetic structures: (a) MO, where M = Mn2+ , Ni2+ , Fe2+ ; (b) MF2 , where M = Mn2+ , Co2+ , Fe2+ . The difference is that the ﬁrst one has a cubic magnetic unit cell with lattice parameter a M twice that of the crystallographic unit cell (a C ), while the magnetic unit cell in the second (tetragonal) structure coincides with the crystallographic

78

ANTIFERROMAGNETISM

Fig. 1. Magnetic structure the antiferromagnets (a) MnO and (b) MnF2 .

one. In most antiferromagnetic materials with

no external magnetic ﬁeld present, M i = 0. However, there exists a large group of antiferromagnetic materials for which this condition is not strictly met. They are materials with weak ferromagnetism (weak ferromagnets), in which M i |M i |. There are also more complicated antiferromagnetic structures, which can not be described in terms of sublattices. They are helical and sinusoidal antiferromagnets (see Modulated magnetic structures, Spin density wave). In both types a preferred direction exists. In the helical structure, the spins of all magnetic atoms in each crystallographic layer perpendicular to the preferred direction are parallel to each other. However, the direction of magnetization of each layer is turned relative to the neighboring ones by some angle ϕ = π/n, where n is typically a noninteger number. In sinusoidal structures, the magnetizations of layers are not parallel to each other, but their value varies according to the law Mk = M0 sin(k ϕ). Both structures are incom-

mensurate in the sense that the magnetic and crystallochemical translational periods are not multiples of each other. In most antiferromagnetic materials, the directions of magnetization vectors M i relative to crystallographic axes are determined by much weaker interactions than the exchange (E ex ) interactions, causing the anisotropy of antiferromagnetic materials (E a ) (see Magnetic anisotropy). The axis along which the magnetizations of sublattices are aligned is known as the easy axis. Antiferromagnetic materials with E a E ex , referred to as metamagnetics, do not exhibit a spin-ﬂop transition (see Magnetic phase transitions). Also referred to as metamagnetics are layered antiferromagnets in which the exchange interaction E ex inside a layer is ferromagnetic and much stronger than the antiferromagnetic interaction between the layers. A direct method to determine the antiferromagnetic structure (including the direction and even the temperature dependences of the sublattice magnetizations) is magnetic neutron diffractometry. The intensity of magnetic diffraction peaks is proportional to the square of the sublattices magnetization. In real antiferromagnetic substances antiferromagnetic domains exist. In weak magnetic ﬁelds, the magnetization M in antiferromagnetic materials, as well as that in a paramagnet, depends linearly on the magnetic ﬁeld (M = χB); however, the temperature dependences of χ in these substances differ signiﬁcantly. In uniaxial crystals the salient features of antiferromagnetism (e.g., anisotropy of magnetic susceptibility) are exhibited most clearly. In particular, the longitudinal (along the antiferromagnetism axis) magnetic susceptibility χ decreases sharply as temperature T decreases, while the transverse one χ⊥ is almost independent of the temperature (Fig. 2). Thus, there is a strong anisotropy of the magnetic susceptibility. If the magnetic ﬁeld directed along the easy axis attains the critical value B c1 = (2B A B E )1/2 (B A is the effective anisotropy ﬁeld), magnetic sublattices ﬂip over in the direction perpendicular to the magnetic ﬁeld. This spin-ﬂop transition occurs because at B > B c1 the difference of magnetic energies in the easy axis and ﬂipped over states becomes greater than the anisotropy energy E A : (1/2)(χ⊥ − χ )B 2 /μ > E A . In samples of ﬁnite

ANTIFERROMAGNETISM

79

Fig. 2. Anisotropy of the magnetic susceptibility χ in an axial antiferromagnet. Fig. 3. Spectrum of spin waves in MnF2 .

size, the intermediate state with alternating layers of ﬂipped over and normal phases is formed in the narrow region of ﬁelds near B c1 due to the energy of demagnetization. There exists a second critical ﬁeld B c2 = 2B E at which the antiferromagnetism is destroyed completely, and all magnetic moments align strictly parallel to the applied ﬁeld (i.e. a spin-ﬂip transition occurs). Other magnetic phase transitions are observed in antiferromagnets as well. A theoretical description of antiferromagnetism can be given within both phenomenological and microscopic models. A phenomenological description based on the Landau theory of secondorder phase transitions uses the expansion of the free energy in even powers of components of magnetization vectors of magnetic sublattices, taking into account the crystal symmetry. This theory predicts symmetries of magnetic phases, as well as the shape of phase diagrams in the vicinity of TN . The microscopic theory uses a Heisenberg Hamiltonian written in terms of spin operators, and leads to the energy of the “ground” state and a spectrum of spin waves. In contrast to ferromagnets, the microscopic theory of Heisenberg magnets faces a fundamental difﬁculty because the state with the strict antiparallel spin alignment is not a true ground state of the system in the presence of an antiferromagnetic exchange interaction. At a ﬁnite temperature T , the quasi-particles that destroy antiferromagnetic order are magnons (spin waves). The existence of several sublattices leads to the existence of several branches, one for each sublattice, of spin waves. Two of them are quasi-acoustic, and the rest are of the exchange

type. The quasi-acoustic spin waves satisfy a linear dispersion law. In most antiferromagnetic materials, however, their spectrum has an energy gap, with the width determined by the expression ω = μB (2B A B E )1/2 , where μB is the Bohr magneton. The existence of the linear dispersion law is conﬁrmed by the linear temperature dependence of the speciﬁc heat, and more reliably by inelastic neutron scattering. Fig. 3 shows the spin wave dispersion relationships of MnF2 . In the scale used, the gap is barely observable. The gap in the spin wave spectrum is studied by means of antiferromagnetic resonance without any particular difﬁculties in easy-plane antiferromagnets where an almost gapless branch is observed, in addition to the magnon branch with a large gap (≈μB (2B A B E )1/2 ). The study of this nearly gapless branch allows the subtle effects of the dynamic interaction of the spin system with other degrees of freedom of the crystal (phonons, oscillations of nuclear spins, etc.) to be revealed. This becomes possible because of the “exchange ampliﬁcation” of the frequency of coupled vibrations in antiferromagnets. Branches of the exchange spin waves are relatively less studied; spin-wave analogues of optical phonons have a wide gap ≈μB B E , and rather weak dispersion. Many antiferromagnetic materials are transparent in the optical and infrared regions. The distinctive features of the optical properties of antiferromagnetic materials are the abnormally high spontaneous magnetic birefringence arising in the easy-plane, and the change of birefringence in the easy-axis antiferromagnetic materials. Singlemagnon scattering also turns out to be stronger

80

ANTIFERROMAGNETISM VECTOR

than what could be expected from the magnetic dipole–dipole transitions alone. Exciton–magnon excitations are observed in the absorption spectra. ANTIFERROMAGNETISM VECTOR A macroscopic parameter of antiferromagnets and ferrimagnets; the order parameter at the magnetic phase transition to the antiferromagnetic state (see Antiferromagnetism). The vector of an-

tiferromagnetism is deﬁned as such a linear combination of the magnetization vectors M α of individual magnetic

sublattices, that it differs from a sum M = kα=1 M α which deﬁnes the total magnetization, where α = 1, 2, 3, . . . , n, and n is the number of sublattices. To describe the atomic magnetic structure, n − 1 antiferromagnetism vectors Li are introduced. The expression for Li depends on the magnetic structure, e.g., in the simplest two-sublattice antiferromagnet (or ferrimagnet), only one such antiferromagnetism vector exists, L = M 1 − M 2 . Sometimes, normalized antiferromagnetism vectors are used, l = L/|L|, l 2 = 1. It is possible to write dynamic equations for the antiferromagnetism vector to deﬁne linear and nonlinear spin waves in antiferromagnets and ferrimagnets (see Landau–Lifshits equation). ANTIFRICTION MATERIALS

Materials having low values of the friction coefﬁcient. Besides low values of the friction coefﬁcient (0.004–0.10 with lubricant, and 0.12–0.20 without lubricant), antifriction materials are characterized by considerable wear resistance, adequate mechanical strength and plasticity, corrosion resistance, and absence of sticking. These materials slightly wear the adjoining surfaces. Depending on the operating conditions antifriction materials with special properties are created to be used with lubrication by oil or water, without a lubricant, in the atmosphere or in vacuo, at a high temperature, in chemical environments, etc. Classiﬁed among antifriction materials are the following: cast materials (babbitts, bronzes, and brasses); baked ones manufactured by powder metallurgy, including composite materials on the base of iron or bronzes; combined (mostly metal-ﬂuoroplastic) materials; antifriction cast irons and antifriction steels (copper steel, graphitized steel). The cast

antifriction materials are manufactured by melting source components with subsequent casting. As to the structure type, they are subdivided into those with harder inclusions of intermetallic compounds placed in a relatively light matrix (e.g., aluminum bronze, tin bronze, tin babbitt), and those with soft inclusions with metallic structural components in a stronger solid solution matrix (e.g., lead bronze, aluminum alloys containing tin, lead and cadmium). A typical feature of baked (metalloceramic) antifriction materials is the presence of pores (8–27% of the volume) which are impregnated with a ﬂuid lubricant. The metallic base of such materials is iron, steel, copper, bronze, and nickel. In addition to these, baked materials contain components (graphite, sulﬁdes, selenides and others) to serve as a dry lubricant. Baked antifriction materials in most cases have higher tribotechnical properties than the ones obtained by casting, and can provide unique properties unattainable in cast alloys. ANTIMONY (Lat. stibium), Sb

A chemical element of Group V of the periodic system with atomic number 51 and atomic mass 121.75. It is related to As and Bi in its properties. Natural antimony has 2 stable isotopes Sb121 (57.25%) and Sb123 (42.74%). Important radioactive isotopes are Sb122 (T1/2 = 2.8 days), Sb124 (T1/2 = 60.2 days), Sb125 (T1/2 = 2.0 years). Electronic conﬁguration of the outer shell is 5s 2 5p3 . Successive ionization energies are 8.64, 16.5, 25.3, 44.0, 55.4 eV. Atomic radius is 0.161 nm; radius of Sb3+ ion is 0.090 nm, of Sb5+ 0.062 nm, of Sb3− 0.208 nm. Work function is 4.08 eV. Oxidation states are −3, +3, +5. Electronegativity is ≈2.0. Antimony is a silvery-white metal with strong brilliance. In a free form antimony exists in several crystalline and amorphous modiﬁcations. Under normal conditions, the rhombohedral crystalline modiﬁcation is stable with parameters a = 0.45064 nm and α = 57.1◦ . Under increased pressure the cubic and hexagonal modiﬁcations appear. Besides, three amorphous modiﬁcations are known: yellow, black and explosive ones. The rhombohedral modiﬁcation is characterized by gray star-like crystals. For this modiﬁcation the density is 6.690 g/cm3 ; Tmelting = 903.5 K,

ANTISCREENING FACTOR

Tboiling = 1907 K. Heat of melting is 20 kJ/mole, heat of evaporation is 124 kJ/mole; speciﬁc heat cp = 25.2 kJ·mole−1 ·K−1 . Thermal conductivity is 18.84 W·m−1 ·K−1 , temperature coefﬁcient of linear expansion of polycrystalline antimony is 9.2·10−6 K−1 (at 273 K), 10.3·10−6 K−1 (at 873 K). Debye temperature is 204 K. Brinell hardness of technical grade antimony is 320 to 580 MPa; of zone reﬁned antimony it is 260 MPa. Shear modulus is 20 GPa, normal elasticity modulus is 56 GPa. Antimony is a diamagnet; magnetic susceptibility of polycrystalline antimony is 0.81·10−9 (at 293 K); electrical resistivity 0.39 μ·m (273 K), temperature coefﬁcient of electrical resistivity is 5.1·10−3 K−1 . Compounds of antimony with indium, gallium, aluminum, cadmium and other metals (so-called antimonides) possess semiconductor properties, with indium antimonide InSb possessing the highest carrier mobility among all known semiconductor materials. Antimony is also used as a component of various alloys, it is contained in lead storage battery plates (4 to 12% by mass). Antimony oxide Sb2 O3 is introduced into the composition of glasses characterized by a low refractive index. ANTIREFLECTION COATING OF OPTICAL ELEMENTS

A means of increasing light transmission of optical elements by coating their surfaces with nonabsorbtive lm s. The optical paths through such ﬁlms should be comparable to the radiation wavelength. Without an antireﬂection coating the loss of light during reﬂection from their optical surfaces may reach 10% or more. The antireﬂection effect involves interference of light beams reﬂected from the front and back sides of the dielectric layers that form the coating. Provided the angles of incidence remain close to normal the antireﬂection coating has a maximum effect. The thickness of the thin coating ﬁlm should be an odd number of quarter wavelengths, and the refractive index of the ﬁlm, n2 should satisfy the relation n22 = n1 n3 , where n1 and n3 are the indices of refraction of the two media adjacent to the ﬁlm (the ﬁrst is often air, n1 = 1). For optical elements made of glass with a low value of n2 a single layer antireﬂection coating is often insufﬁcient, whereas

81

two-layer coating ﬁlms almost totally eliminate ree ction of light from the surfaces of the optical elements. Note that this is true in a rather narrow spectral range only. To attain antireﬂection protection over a broad spectral range triple and multiple layer coating systems are commonly used. Antireﬂection coating plays a very important role in lowering optical losses in multilens optical systems, in laser technology where coating makes it possible to lower feedback losses from the optical cavities, in opto-acoustic instruments, etc. ANTIRESONANCE, MAGNETIC See Magnetic antiresonance. ANTIRESONANCE, OPTICAL See Optical antiresonance. ANTI-SCHOTTKY DEFECT A two-component defect in crystals of binary

(MX) or more complex composition. Its components are IM and IX , the amounts of interstitial atoms of chemical elements M and X which themselves constitute the regular lattice of the crystal. Anti-Schottky defects can be equilibrium stoichiometric defects arising at elevated temperatures, e.g., because of “vaporization” of M and X atoms from the surface to the inside of the MX crystal. The creation of anti-Schottky defects is hampered by the necessity of inserting the larger M and X atoms into the smaller-sized interatomic “cavities” (i.e. interstitial sites). These defects have the name anti-Schottky because a Schottky defect is a vacancy formed by transferring an atom from the bulk of the crystal to its surface. ANTISCREENING FACTOR

A parameter characterizing antiscreening (the phenomenon which is inverse to electric charge screening). If P0 is a response arising as a result of some inﬂuence in the absence of a medium, and P is the same response in the presence of the medium, then one can write P = P0 (1 − γ ). If the dimensionless parameter γ is less than zero it is commonly referred to as an antiscreening factor. The Sternheimer antiscreening factor (R.M. Sternheimer, 1951) γ S describes the enhancement of an intracrystalline electric ﬁeld gradient at a nucleus

82

ANTISITE DEFECT

due to the polarization of closed atomic shells by external electric charges. The value of |γ S | can be rather large (50–100). ANTISITE DEFECT

An atom of one sublattice of a two- or multicomponent crystal, occupying a site of another sublattice; actually, a substitutional atom, denoted as XM (atom X at a site of sublattice M). Adjacent defects XM and MX represent an antistructural defect pair. For unequal concentrations of MX and XM the antisite defects determine an excess of component M or X, i.e. a deviation from stoichiometric composition. ANTI-STOKES LUMINESCENCE Photoluminescence, or luminescence at wave-

lengths less than that of the exciting light, which is in contradiction with Stokes’ rule. Anti-Stokes luminescence is common in the region of overlap between the excitation and the luminescence wavelengths. The emission of a quantum with an energy exceeding that acquired in the absorption occurs due to the additional involvement of the thermal motion of the luminescent system. This results in the Vavilov law, which reﬂects the fact that the probability of such a process decreases rapidly as the involved energy rises, and it depends on the thermal motion intensity (temperature). Of greater importance are the fundamental violations of Stokes’ law when the emitted luminescence lies in the region of wavelengths less than that of the exciting light. Such effects are possible by making use of several exciting light quanta (most often, of two) in the emission process, by the simultaneous absorption of two photons by one electron at a high excitation intensity, by sequential absorption of two quanta by the electron, and by pooling the energy of two excited electrons to produce the emission (cooperative luminescence), etc. ANTI-STOKES RAMAN LINES Lines in the spectrum of Raman scattering of light that are located on the high-frequency side of

the exciting line. Anti-Stokes light scattering lines are caused by annihilation of the excitation quantum in the system by the inelastic scattering of an incident photon on it (a phonon, magnon, plasmon, etc., is typically annihilated in a crystal). The intensity of

anti-Stokes lines depends on the initial level population (excited) and decreases with a lowering of the temperature. The presence in a spectrum of Stokes and anti-Stokes pairs of lines, symmetric relative to exciting one, is often used to discriminate between the processes of Raman scattering and luminescence, while their intensity ratio characterizes the scattering medium temperature. ANTISTRUCTURAL DEFECT A defect in a binary or more complex crystal

containing two chemical elements M and X. The defect consists of two components – substitutional atoms MX (atom M at site X) and XM (atom X at site M). The formation of antistructural defects in a nonmetallic crystal can be accompanied by changing the charge state of its components. For example, atoms M and X in the normal positions at their “own” sites MM and XX can be neutral, while as components of an antistructural defect, if M is a metal, MX tends to become an acceptor and X (metalloid) a donor XM . Antistructural defects either exist in the equilibrium state at elevated temperatures (e.g., in crystals Bi2 Te3 , Mg2 Sn, and others) or are created as nonequilibrium metastable defects, e.g., as a result of nuclear radiation (see Antisite defect). ANTISYMMETRIC VIBRATIONS of crystal lattice Normal vibrations which reverse their sign un-

der the application of an appropriate symmetry operation (see Crystal symmetry). In ionic crystals antisymmetric vibrations involve a change of the electric dipole moment. ANTISYMMETRY of crystals, Shubnikov symmetry One of the particular cases of colored symmetry (hypersymmetry). In ordinary crystal symmetry, only spatial (position or orientation) symmetry

is considered, while in hypersymmetry, another attribute (conventionally, color or spin direction) is assigned a value at every point of the crystal. If the additional attribute can take on only two alternative values (black and white), such a particular case of hypersymmetry is referred to as antisymmetry, in other words as black and white symmetry. If there are many values then one speaks

ARMCO IRON

about color symmetry. Another term for antisymmetry is Shubnikov symmetry after A.V. Shubnikov who introduced the concept. In analogy to the ordinary crystal symmetry groups, there exist 122 point, 36 translational and 1651 space Shubnikov groups. All of them have been derived and classiﬁed, a system of notation has been developed, and they are used in concrete physical studies. Examples of the physical realization of crystal antisymmetry can vary. Treated as the color change operation may be, for example, a change in the chemical type of atoms in an ordered binary alloy, or in the sign of the displacement of atoms and of the electric charge, and others. Solid state physics makes the widest use of this approach for the Shubnikov classiﬁcation of the magnetic symmetry of crystals, where the color change operation has the sense of the time inversion operation R, and, as a consequence, the inversion of the magnetic moments and magnetic elds (see Magnetic symmetry group). Operations of antisymmetry, which occur in magnetic crystal symmetry and are combinations of rotation or translation with R, are referred to as antirotations and antitranslations. ANYONS (fr. any)

Particles that obey a statistics which is intermediate between the Bose (see Bose–Einstein statistics) and Fermi (see Fermi–Dirac statistics) types. Such particles can exist in two-dimensional space since the topology of this space admits the presence of indeterminate wave functions for (identical) particles a with strong short range repulsion (hard core). These functions obey the permutation rules Pj k ψ = exp(iπα)ψ , where Pj k means the permutation of j th and kth particles, and α is any real number which is sometimes called a statistical parameter. The value α = 0 corresponds to bosons and α = 1 denotes fermions (see Second quantization), while intermediate values are indicative of an intermediate statistics. The possibility of the existence of an intermediate type statistics was ﬁrst pointed out by J.M. Leinaas and J. Myrheim (1977), and the term “anyon” was introduced by F. Wilczek (1982). Intermediate statistics can also be obeyed by particles in one-dimensional space (to which a term “anyon” is inapplicable, as a rule), and by distinguishable particles (anyons of

83

many types). The permutation conditions for the latter have the form Pj2k ψ = exp(iπα)ψ , and at α = 0, 1 one can speak about an in-between statistics. The ambiguous nature of anyon wave functions results in the fact that the quantum-mechanical problem of many anyons cannot be solved even for the simplest case when there is no interaction. The usual procedure of seeking solutions in terms of single-particle wave functions is not applicable here. The statistics of all elementary particles is determined by their spin in accordance with the Pauli principle. Therefore (since real space is threedimensional), elementary particles with an intermediate statistics cannot exist in free space; this statistics can be valid only for quasi-particles in quasi-two-dimensional and quasi-one-dimensional systems. In particular, the elementary excitations in the fractional quantum Hall effect (see Quantum Hall effect) obey intermediate statistics, i.e. they are anyons. At a ﬁlling factor ν = 1/q where q is an odd integer, the statistical parameter of these excitations is α = ν. The appearance of the effect at ﬁlling factors ν = p/q kept constant is explained quite well in the framework of so-called hierarchic theory. This implies that there appear excitations over a “primary” electron gas that represent the anyon gas. Other excitations can arise which also represent the anyon gas but with another statistical parameter, and so on inﬁnitely. One can demonstrate that under particular conditions an anyon gas is a superconductor. As far as it is known high-temperature superconductivity is of a quasi-two-dimensional nature, and an hypothesis about an anyon mechanism of superconductivity has been suggested, but there is no experimental conﬁrmation of it. See also Anderson mechanism of high-temperature superconductivity. APW METHOD See Augmented plane waves method. ARMCO IRON (ARMCO is an acronym of American Rolling Mill Corporation) Highly puriﬁed iron with high plasticity, enhanced electrical conductivity, high magnetic saturation and resistance against corrosion. ARMCO iron falls into soft magnetic materials, its magnetic

84

AROMATIC COMPOUNDS

properties depending upon the quantity of impurities, sizes of crystal grains, elastic and plastic stresses. ARMCO iron is used for the manufacture of electrical engineering products to be operated in constant and slowly varying magnetic ﬁelds. In metallurgy, it is employed as the basic element in the manufacture of many magnetic alloys and as the charge in the production of alloyed steel. AROMATIC COMPOUNDS

A group of organic compounds possessing a system of conjugated π -bonds. The term originated from the speciﬁc odor of natural substances containing aromatic compounds. These compounds are exempliﬁed by the polycyclics – benzene (C6 H6 ), naphthalene (C10 H8 ), anthracene (C14 H10 ), tetracene (C18 H12 ), pentacene (C22 H14 ), and others, with a common formula C4n+2 H2n+4 , where n is the number of benzene-type rings. The molecules of polycyclics are planar and form molecular crystals in the solid phase. Most of them belong to the monoclinic system with two molecules in a unit cell. Electronic properties of aromatic compounds are determined mainly by pz electrons of C atoms forming a delocalized π -orbital. The π -electrons excited by light undergo a π –π ∗ transition and account for the absorption spectral shift from the ultraviolet to the visible part of the spectrum in the above-indicated sequence of polyacenes. The mobility of π -electrons determines important physical and chemical properties of aromatic compounds: photoconductivity of their crystals, migration of electron excitation energy, catalytic activity. Aromatic compounds are model systems for organic semiconductors. The dark electrical conductivity of pure crystals is low, σ ∼ 10−2 –10−12 −1 cm−1 . The typical mobility of excess electrons and holes moving in narrow bands takes on values of the order of 1 cm2 ·V−1 ·s−1 . ARRHENIUS LAW (S. Arrhenius, 1889)

Relation stating the temperature dependence of the reaction rate constant K U , K ∼ K0 exp − RT where U is the activation energy of the reaction, and R is the universal gas constant. The parameter

Activation energies U1 and U2 for a double minimum potential.

K0 has a temperature dependence weaker than exponential. The value of K is determined from the expression for the reaction rate nA+mB+lC+· · · which is proportional to the product of the appropriate powers of concentrations (denoted by brackets): v = K[A]n [B]m [C]l · · · . The Arrhenius law was deduced empirically and can be justiﬁed from the Boltzmann distribution. The ﬁgure schematically presents the dependence of the energy of the reacting particles on their generalized coordinate. The activation energies U1 of the reaction 1 → 2 and U2 of reaction 2 → 1 are determined by the energies of the initial states 1, 2 and the height of the potential barrier separating them. The barrier energy U varies from several electron-volts to almost zero; it can equal zero, e.g., in ionicmolecular reactions or in the reactions with mechanisms based on the tunnel effect. Such reactions can occur at temperatures close to absolute zero. Reactions in solids with participation of the inherent and impurity atoms, conduction electrons, and various quasi-particles also follow the Arrhenius law. In them, a part of the activation energy U D can arise from the diffusion of reagents, determined by the temperature dependence of the diffusion coef cient D = D0 exp(−U D /RT ). See also Interdiffusion, Activation energy, Thermal activation. ARTIFICIAL EPITAXY See Amorphous epitaxy.

ASTERISM

ASBESTOS (fr. Gr. ασβεσ τ oς , unquenchable) Fine-ﬁber minerals capable of splitting into

ﬂexible and thin ﬁbers (up to 0.5 μm thick). The most signiﬁcant is serpentine asbestos. There are such varieties as chrysotile-asbestos and picrolite. Chrysotile-asbestos Mg6 Si4 O10 (OH)8 has a lamellar-tubular structure with a monoclinic lattice. Felted and parallel-ﬁber aggregates are typical of it. The cleavage is imperfect along (110) at the angle 130◦ . Density is 2.5 to 2.65 g/cm3 . Mohs hardness is 2.0 to 3.0. Impurities: Fe (up to 3%), Ca, Mn, Ni, Al, Na. Water content is 13.0 to 14.8%. Refractive indices: ng = 1.522 to 1.555; np = 1.508 to 1.543. The ﬁbers of asbestos are rupture-strong (285 to 365 kg/mm2 ). Asbestos is ﬁreproof (T melting is 1500 ◦ C); it has high sorption ability (see Sorption), swelling ability; it conducts heat poorly; it is stable against alkalis; upon heating, it loses water and transforms to forsterite. Asbestos is used in textile, cement, paper, radio industry, road surfacings, etc. ASCENDING DIFFUSION

A process of transport, whereby the ﬂow of particles is directed along the concentration gradient. In contrast to conventional diffusion, in this case the difference in concentration of the diffusing component does not diminish but rather grows. The possibility of ascending diffusion arises from the fact that the driving force of the diffusion is the gradient of the chemical potential which, in general, can differ from the concentration gradient. Different ﬁelds which contribute to the chemical potential in addition to the entropy of mixing, can cause the ascending diffusion; examples are thermal ﬁelds (thermodiffusion), electrical ﬁelds, vacancy ﬁelds, phase non-uniformity of the material, and the ﬁeld of elastic stresses. These ﬁelds make the potential barrier that the diffusing particle encounters an unsymmetrical one, and the result is a preferred drift in the direction of the ﬁeld. In a general phenomenological theory ascending diffusion can be described in a systematic uniform manner, but the detailed mechanisms operating in the above mentioned cases are different. The Gorsky effect (V.S. Gorsky, 1935), which involves ascending diffusion caused by local gradients of elastic stresses in crystals, is speciﬁc for solids. For example, during the bending of a plate

85

made of metal alloys the concentration of atoms with the greater atomic radius grows at the exterior side of the ﬂexure (a partial stress relaxation accompanies this process). By providing for the segregation of atoms of different types, ascending diffusion, evidently, plays an important role in the phase separation in alloys, and at the formation of atmospheres of the impurity atoms in the strained regions of a crystal, e.g., interstitial atoms preferentially concentrate in the stretched region of the ﬁeld of stresses at dislocations (see Cottrell atmosphere). ASPEROMAGNET An amorphous magnetic substance in which the random frozen magnetization mi has a ﬁrst

moment M = mi c and two second moments, 2 q = (mi )2 c and q⊥ = (m⊥ i ) c . The averaging is performed over conﬁgurations, the indices and ⊥ denoting projections of mi onto the vector M or onto the plane perpendicular to M, respectively. The asperomagnetic state is observed in two types of amorphous magnetic materials: in alloys and metallic glasses containing rare-earth elements and noble metals, such as DyCu, TbAg; in systems of the spin glass type. In the ﬁrst case, the origin is the large value of the magnetic anisotropy constant (typical of rareearth elements) and the random orientations of the anisotropy axis (typical of alloys and glasses). In the second case, the cause is the presence of concurrent random ferro- and antiferromagnetic interactions. Asperomagnets often exhibit nonergodic behavior (see Nonergodicity). ASTERISM

The characteristic oblong shape of X-ray diffraction spots from deformed monocrystals exposed to X-radiation of a continuous type. In the case of transmission images (Laue patterns), the diffraction spots are elongated toward the center of the picture. Asterism arises due to the reﬂection of the X-ray beam from the bent part of a crystal. The horizontal diameter of the spot in angular units is ϕ1 = 2α and the vertical one is ϕ2 = −2α sin θ , where θ is the Bragg angle (see Bragg law) and α is the ﬂexure angle of the reﬂecting plane. At small θ , ϕ2 ϕ1 which explains elongation of spots at asterism, and proves that the

86

ATHERMIC CREEP

length of asterism bands can serve as a measure of e xure. In reﬂection imaging (epigrams), the directional stretching of diffraction spots is observed according to the ﬂexure axis orientation relative to the initial beam. ATHERMIC CREEP

A type of low-temperature logarithmic creep, independent of temperature. Its rate after the instant jump of the initial strain ε0 at the moment of load application quickly decreases in time, ε = α/t . Typical for this creep is the time dependence of strain caused by the motion of dislocations, ε = ε0 + α ln(νt + 1), α and ν being constants. A feature of athermic creep is the smallness (0.1 to 1%), in comparison with ε0 , of the strain under creep. The deceleration of athermic creep is associated either with the increasing density of support of intersecting dislocations or with the “depletion” of mobile dislocations. At temperatures close to absolute zero (∼1 K), the barriers of the support type are overcome with the help of a quantum-mechanical tunnel effect (see Lowtemperature yield limit anomalies). According to Mott, in this case α is independent of temperature, α ∝ 2πh/(2Mu)1/2 , where h is the Planck constant, M is the effective mass of dislocations, u is a quantity on the order of the energy of the step transformation at the dislocation (3·10−19 J). Within the range of temperatures between 1 K and T ∼ 0.1Θ, where Θ is the Debye temperature, the crossing of the support may be activated by zeropoint vibrations of dislocation segments. The factor 2 T 1 kBΘ 1+ α= 2 hν Θ insigniﬁcantly changes with temperature at T < Θ. The value of ε at the athermic creep is not large, but it needs to be accounted for in the operation of precision parts and products. ATHERMIC PLASTICITY

Lack of sensitivity of the characteristics of a plastic deformation process of a solid to changes

in temperature. Athermic plasticity characterizes the regularities of plastic deformation of crystals at low and

very low temperatures. It emphasizes that the thermoactivating character of elementary dislocation processes in determining the deformation kinetics, such as overcoming Peierls barriers by dislocations (see Peierls–Nabarro model) or local barriers determined by the defects of crystalline structure, is of limited applicability for the description of low-temperature plasticity. Athermic plasticity is not fully understood; it has been proposed as (i) playing a crucial role in quantum ﬂuctuations that arise during the motion of dislocations through barriers, and (ii) playing a role in the replacement of a thermoactivated barrier penetration by an activation-free process of the overbarrier motion, which occurs owing to the high level of effective forces acting upon dislocations, and the low level of dynamic friction restraining the dislocations (see Internal friction), typical for low-temperature deformation. ATMOSPHERE See Cottrell atmosphere, Snoek atmosphere, Suzuki atmosphere. ATOM

An atom consists of a positively charged nucleus with a size on the order of 10−15 m and a surrounding electronic cloud with a size of about 10−10 m (see Atomic radius). An atom as a whole is electrically neutral; the positive charge of the nucleus Ze (Z is the atomic number and e is the elementary electron charge) is compensated by the negative charge of its Z electrons. An atom can accept or donate one or more electrons to become, respectively, a negatively or positively charged ion. The complicated structure of the electron cloud is determined mainly by Coulomb interactions, the attraction of electrons to the nucleus and their mutual repulsion, as well as by the Pauli exclusion principle. Relatively small but fundamentally important contributions to the energy arise from the spin–orbit interaction and the spin–spin interaction. A single-electron approximation is widely used to describe an atom: the wave function of the electrons is a product of one-electron wave functions (Hartree method) or a linear combination of such products which satisﬁes the requirement of interchange invariance (Hartree–Fock method).

ATOMICALLY CLEAN SURFACE

In this approximation one can speak about oneelectron energy levels and corresponding electron shells of an atom. To describe them approximately, the model of a hydrogen-like atom is employed, with the shells characterized by the principal quantum number n = 1, 2, 3, . . . , and their substructure by the orbital quantum numbers l = 0, 1, 2, . . . , n − 1 and m = 0, ±1, . . . , ±l. The electrons of the K-shell with n = 1 are closest to the nucleus with the deepest (most negative) energy levels. Then follow the L, M, N, . . . shells with n = 2, 3, 4, . . . . In the ground states of the atoms H and He only the K-shell is occupied. As Z grows, the orbits with higher quantum numbers become ﬁlled. The electron conﬁguration of an atom is speciﬁed by symbols that indicate the values of quantum numbers n and l of ﬁlled shells in ascending order, and the number of electrons in them; the values l = 0, 1, 2, 3, 4, . . . being denoted with corresponding letters s, p, d, f, g, . . . . For example, the conﬁguration 1s 2 2s 2 2p6 of the neon atom has two electrons with n = 1 and l = 0, plus two electrons with l = 0, and six electrons with l = 1 at n = 2. Each l shell contains 2(2l + 1) electrons when it is full. Another approximate method for describing an atom (Thomas–Fermi method) is based upon a structureless cloud of atomic electrons with their density distribution determined by the Poisson equation. The outer valence electrons determine the chemical properties of atoms, their ability to form this or that compound, the structure, binding energy, and other characteristics of compounds. Although atoms are the structural elements of solids, the distribution of the atomic electrons in a solid differs from that of a free atom. The conﬁgurations of valence electrons undergo considerable changes, depending on the type of bonding force between atoms, the number and positions of nearest neighbors, etc. In a crystalline solid, the states of valence electrons depend on whether the atoms occupy sites of the regular lattice, or they are doping atoms or substitutional atoms. The presence of the two latter types introduces additional levels in the energy spectrum of electrons in crystals and inﬂuences the optical, electrical and other properties of a crystal. The inner atomic shells also undergo some change, but to a much lesser extent. This

87

is substantiated by data of X-ray emission spectroscopy, by the observed differences of characteristic X-ray frequencies for the inner shells of atoms of a given chemical element incorporated into different chemical compounds. It is not feasible to solve exactly the problem of the states of atoms forming (comprising) a solid. The approximation often used in condensed matter theory is based on reducing the number of independent variables per atom down to 3. Here, the atom is represented as a structureless entity, while interactions involving atoms are described by various, mostly empirically chosen, potentials with limited applicability (see Interatomic interaction potentials). In a more precise approach the valence electrons are singled out, and the nucleus with the deep electron shells is treated as a point particle with an effective charge. The potential of an atom is determined by the distribution of its electron density. An approaching test particle perturbs this distribution in a manner that depends on its nature and its speed relative to the atom. Atom–atom potentials differ for different pairs of atoms. In the quantum description one cannot speak about each particular electron being afﬁliated with one particular atom of a solid. The delocalization of electrons among many atoms causes the splitting of atomic energy levels and the creation of bands of allowed energies in crystals. Such broadening is rather small for electrons in deep levels. For those in outer atomic shells, broad (several electron-volts) allowed energy bands arise, and are particularly prominent in metals, with their structure determining the electric, optical, and other properties of the crystal. ATOM DISPLACEMENTS See Static displacements of atoms, Thermal displacements of atoms. ATOMICALLY CLEAN SURFACE

A surface free of impurities and having a pristine crystal structure. To obtain and preserve an atomically clean surface, various methods of cleaning in a super-high vacuum (10−8 Pa) are used. The main methods are high temperature heating, bombardment with ions of noble gases with annealing and chemical pretreatment to obtain products that are removable at

88

ATOMIC CHARGE

moderate temperatures. An absolutely clean surface is impossible to obtain: the sources of contamination are the impurities in a crystal bulk and the adsorption of particles from residual gases. Therefore, the surface is considered to be clean, if the concentration of impurities is so small that it fails to affect phenomena under study. Auger electron spectroscopy is the most suitable method of monitoring surface cleanliness (the sensitivity is 10−2 –10−3 monolayers). The investigation of an atomically clean surface structure is performed by low-energy electron diffraction and high-energy electron diffraction methods (see Electron diffraction). From an analysis of the data from structural investigations, the atomically clean surfaces of crystals, especially semiconductor ones, can be reconstructed. Surface structures can form with periods other than those in atomic planes in a crystal bulk parallel to the surface. A special notation is adopted for these surface structures. They include the chemical symbol of the crystal, the orientation of a face, and the ratio of the unit cell vectors of surface structure to the corresponding vectors in the bulk, e.g., Si (111) – 7 × 7, Au (100) – 5 × 1 and so on. According to modern concepts, the cause of the reconstruction of the upper atomic planes of a crystal is the tendency to reduce the excessive free energy of a surface lattice relative to that in the bulk. The supposition that the reconstruction is determined by the uncontrollable contamination of a surface failed to be conﬁrmed experimentally. The difﬁculties connected with clariﬁcation of the nature of surface reconstruction are complicated by the fact that the problem of the determination of the coordinates of the unit cell atoms for the surface structures with large unit cells is yet to be solved because of the complexity of the calculations in the structural analysis. Therefore, various hypothetical models are used in discussions of this reconstruction, their ability to approximate reality being tested using data obtained by various methods. All the varieties of models can be divided into two classes: those based on small static displacements of atoms from their normal positions in the surface lattice, and those involving the concept of orderly-spaced defects at the surface (vacancies, adatoms, etc.). There has been considerable progress in understanding surface structures

because of data obtained from scanning tunneling microscopy. According to estimates based on different data, the reconstruction encompasses several atomic planes of a crystal. There are only a limited number of orientations of planes which coincide with atomic planes having the same crystallographic indices and characteristic surface structures. Such surfaces are referred to as atomically smooth. In other cases, energy can be gained by the decay of a ﬂat surface to micro facets, or by the formation of a stepped surface including terraces of low-index facets connected by equispaced atomic steps as high as one or more interplane distances. Besides the structure, there are also other important properties of a surface such as the electronic energy band structure and dynamical characteristics (frequencies of atomic vibrations, their vibration amplitudes) that are different from the analogous properties in the bulk. Therefore, the near-surface region is considered as a special surface phase with its own conditions of equilibrium. The atomically clean surfaces of some crystals of semiconductors and metals with particular orientations are the place where order–disorder phase transitions as well as order–order ones occur, while there are no phase transitions in the bulk. The order–order reconstruction can occur as transitions between surface structures, both with unit cells lying in one plane, and with changes of facet structure – morphological transitions. ATOMIC CHARGE See Effective atomic charge. ATOMIC FORM FACTOR

A parameter of the elastic scattering of a plane wave (X-ray, electron, neutron) by an isolated atom, which determines the amplitude of the scattered wave as a function of the scattering angle. In the scattering of waves in crystals, the amplitudes of scattering by individual atoms are ampliﬁed in some directions, while they are decreased in others; the total result being determined by the values of the atomic form factors of the atoms forming the crystal. A general expression for an atomic form factor is f (s) = K ρ(r) exp(is · r) dr ,

ATOMIC MAGNETIC STRUCTURE

89

types that correspond to ferromagnetism, antiferromagnetism, and ferrimagnetism.

Atomic form factor.

where s = k − k 0 , and k 0 , k are the wave vectors of the incident and scattered waves, respectively (see Fig.), and K is a factor dependent on the type of radiation. The X-ray scattering is determined by the electron density ρ X = |ψ(r)|2 , and values of f X (s) are on the order of 10−11 cm. The electron scattering is determined by the electrostatic potential of the atom ϕ(r); ρ el (r) = ϕ(r), with values of f el (s) of the order of 10−8 cm. Neutron scattering may be thought of as taking place at the point potential of the atomic nucleus, with values of f n (s) of the order of 10−12 cm, and no angular dependence. ATOMIC MAGNETIC STRUCTURE

Position and spatial orientation of atomic magnetic moments, or of the magnetic moment density of delocalized electrons (the latter pertains to band magnetism). The presence of a magnetic structure in a material implies that the time averages of the above quantities differ from zero. These averages are zero in materials having no magnetic structure (an external magnetic ﬁeld is presumed absent). The emergence of a magnetic structure in a material is always accompanied by symmetry lowering, if for no other reason than that the time reversal operation is not a symmetry transformation. In this connection, the state of a material exhibiting a magnetic structure is called a magnetically ordered state, and the process of transforming to a magnetically ordered structure is a magnetic phase transition of the disorder-to-order type. A magnetic structure is commonly found in those crystalline substances where the magnetic atoms tend to occupy symmetrical crystallographic sites, while the mean magnitudes of atomic magnetic moments are oriented in a deﬁnite manner with respect to one another and to the crystallographic axes. The magnetic structure of most magnetic crystals can be classiﬁed as one of three basic

A ferromagnetic structure refers to one with all the magnetic moments aligned in the same direction. This structure is characterized by the magnitude and direction of the magnetization M. The simplest antiferromagnetic structure is a set of two interpenetrating magnetic sublattices, with their respective magnetization vectors, M 1 and M 2 , equal in magnitude and opposite in direction, viz., the net vector M = M 1 + M 2 is zero. The two-sublattice antiferromagnetic structure is described by the magnitude and direction of the antiferromagnetism vector, L = M 1 − M 2 . The condition M 1 = −M 2 necessarily assumes that atoms belonging to different magnetic sublattices are the same, and their crystallographic positions are equivalent, since a difference in the magnetic moments inevitably results from the dissimilarity of the atoms, or their positions. More complicated antiferromagnetic structures have been discovered in many crystals. For example, in Mn3 NiN, the magnetic moments are directed along the sides of an equilateral triangle (a non-collinear antiferromagnetic structure with three sublattices), while in YMnO3 , they follow the directions of the sides of two equilateral triangles rotated by 60◦ relative to one another (a six-sublattice structure). Noncoplanar antiferromagnetic structures are also encountered, e.g., the magnetic moments in the foursublattice antiferromagnet UO2 lie along the body diagonals of a cube. Any particular magnetic structure of the ferroor antiferromagnetic type forms in a substance as a result of electrostatic exchange or direct interactions, with the exchange interactions far exceeding, as a rule, those of the direct type (i.e. magnetic dipole interactions and spin–orbit interactions). In quite a number of materials exchange interactions establish an antiferromagnetic structure (a bi- or polysublattice one), whereas the other interactions (see Dzialoshinskii interaction) bring about a small distortion of this structure, which causes a nonzero ferromagnetism vector, M L, to appear. Such materials are called weak ferromagnets, and the corresponding magnetic structures are called weak ferromagnetic structures. The competition of the strong electrostatic and weak direct forces may also have other conse-

90

ATOMIC ORBITALS

quences i.e. it may produce a long-period modulated magnetic structure in a crystal. Here, the exchange forces order the magnetic moments according to either a ferro- or antiferromagnetic pattern, while the relativistic forces lead to the vectors M = M(ξ ) or L = L(ξ ) gradually changing along a certain direction ξ that is called the axis of the modulated structure. In the simplest modulated structures, M (or L) just rotates around the axis (long period helices); there are also more complicated modulated magnetic structures. The formation of a magnetic helix in some crystals is due to the exchange interaction. The helix period is of the same order of magnitude in this case as the distance between neighboring magnetic atoms. A magnetic helix differs fundamentally from a noncollinear antiferromagnetic structure (e.g., of YMnO3 type) in that the angles between the magnetic moments may not correspond to 360◦ /n values (n = 1, 2, 3, . . .). The helix period is not commensurate with the interatomic distances ξlm in this case. Another common type of magnetic ordering (ferrimagnetic structure) occurs in ferrimagnets, where the exchange forces position the atomic magnetic moments in a manner resulting in nonzero values of both M and L. In particular, a ferrimagnetic structure appears when the magnetic atoms occupy crystallographic positions of two different types, with each type constituting a magnetic sublattice. Magnetic structures of a special type, impossible in magnetic crystals, have been discovered in chemically disordered solid solutions (alloys) (see Amorphous magnetic substances, Spin glass, Asperomagnet). A particular form of modulated magnetic structure, the spin density wave whose period may be incommensurable with the crystal lattice period, may appear in a system of delocalized electrons. All the above magnetic structures have been observed in a number of materials, such as those involving 4f -elements and their alloys (see Magnetism of rare-earth metals), as well as actinidecontaining compounds. There is still another form of magnetic structure called the antiphase domain structure which possesses an alternating sequence in space of the groups of n1 atoms with the magnetic moments oriented along a certain axis, and of the groups of n2 = n1 atoms with opposite

magnetic moment orientations (e.g., in thulium, n1 = 4, n2 = 3). ATOMIC ORBITALS See Orbitals. ATOMIC ORDER on a crystal surface

The ordered arrangement of surface atoms (ions, molecules) that corresponds to a minimal free energy (see Thermodynamic potentials) of a ﬁnite crystal. The order is determined by the interaction of surface atoms with one another and with bulk atoms. It can differ from the arrangement in atomic planes inside a crystal, but parallel to the surface (see Surface superlattice, Surface reconstruction). The possible symmetry types of periodic surface structures are described with ﬁve parallelogram systems of equivalent points (twodimensional analog of Bravais lattices, see Twodimensional crystallography) with primitive unit cells in the shape of a general parallelogram, rectangle, square, rhombus with angle 120◦ , rhombus with angle unequal to 120◦ (in this case, one usually chooses a centered rectangle as a nonprimitive cell). Sometimes, the equilibrium state of a crystal surface is in correspondence with the ordered arrangement of vacancies, adsorbed atoms, atomic steps and terraces on it, e.g., a system of equidistant atomic steps of the same height on the facets with high Miller indices (see Crystallographic indices) in silicon and germanium. The results of surface structure studies by scanning tunneling microscopy, and by low-energy electron diffraction, indicate the presence of atomic order on a crystal surface. ATOMIC RADII

The approximate sizes or radii r a of particular atoms in crystals, assuming them to be spheres touching each other. A typical interatomic spacing between two atoms in a crystal is the sum of their atomic radii. In neutral atom crystals such as solid argon the electron density distribution of outer shells of atoms displays a relatively weak dependence on their nearest neighbors. The value of the outer shell radius averaged over the sphere, which characterizes the atomic size, varies with

ATOM–SURFACE INTERACTION

changes in the chemical composition of the nearest neighbors by a few percent when the number of neighbors (referred to as the coordination number k) is the same, and it varies by up to 10–12% in compounds with different coordination numbers. Common coordination numbers are k = 12, 8, 6, and 4 for face centered cubic (fcc), body centered cubic (bcc), simple cubic (sc) and diamond (ZnS) structures, respectively. Thus, an approximate additivity rule exists: d(AB) = r a (A)+r a (B), where d is the closest distance between atoms A and B in the compound AB, and the r a are their atomic radii. In view of the approximate character of the additivity rule, there is some indeterminacy in the choice of numerical values of atomic radii, and several systems of atomic radii exist. All of them, however, predict values of interatomic distances in crystals with a good accuracy, which has been conﬁrmed with many compounds. The metallic atomic radii r M for k = 12, 8, 6, and 4 are in the ratio 1 : 0.98 : 0.96 : 0.88. The atomic radii for Li, K, Al, Fe, Au are 1.55, 2.36, 1.43, 1.26, 1.44 Å. To describe ionic compounds ionic radii r i are used; with the closest distance between two ions of opposite sign assumed to equal the sum of their ionic radii. Underlying the determination of r i are the radii of ﬂuoride (F− ) and oxygen (O2− ), which are adopted to be r i (F− ) = 1.33 Å, r i (O2− ) = 1.32 Å in the Goldschmidt system and r i (F− ) = 1.36 Å, r i (O2− ) = 1.40 Å in the Pauling system. The concept of atomic radii can be extended to other cases. Covalent atomic radii r c are characterized by a noticeable dependence on the bond multiplicity. The value r c for the atoms C, N, O, S reduces by 12–14%, if two pairs of electrons take part in the bond, and by 20–22%, if three, relative to a single electron pair covalent bond. The covalent atomic radii of C, Cl, Br are 0.77, 0.99, 1.14 Å. In molecular crystals, the additivity condition is approximately met for distances d between the nearest atoms of neighboring molecules. One can introduce a system of intermolecular atomic radii r V (also referred to as van der Waals atomic radii). Due to the relative weakness of their bonding forces, the values of r V are greater than those of atomic radii for strong bonding. For He, C, Cl, Kr, r V = 1.40, 1.70, 1.78, 2.02 Å.

91

ATOMIC STEPS on a surface

Raised boundary regions in a monocrystal that are transitions between terraces – ﬂat regions of atomically smooth surface (see Atomically clean surface). The steps are as high as one or several interplanar distances. As distinct from analogous steps of macroscopic size with a height of several micrometers and more, depending on the extent of a surface treatment, the atomic steps cannot be observed with an optical microscope, but are detectable using low-energy electron diffraction and are observable with an electron microscope, a scanning tunneling microscope, or an atomic force microscope. In experiments involving the reﬂection of heavy ions with energy 1–50 keV under grazing incidence on a monocrystal surface with a variation of the angle of incidence, the scattering by the atomic steps “upward” and “downward” (relative to the incident beam direction) produces characteristic features in the energy spectrum of the scattered ions, and marked differences in the extent of their ionization. This allows the use of the scattering of medium energy electrons to diagnose the step structure of a solid surface at the atomic level. ATOMIC STRUCTURE OF A SURFACE See Surface atomic structure. ATOM–SURFACE INTERACTION The interaction of atoms that is deﬁned by

characteristic features of their position on the surface. The crystal surface has an excess of energy compared to the bulk. The coordination number of surface atoms is less than that of the atoms in the bulk (see Coordination sphere), which causes the appearance of uncompensated elastic forces acting on the surface atoms. The formation of a surface can be accompanied also by the appearance of atomic dipole repulsive moments caused by the shift of electron clouds into the depth of a crystal due to the electric potential jump on the surface. The effect of these factors is that the dynamical characteristics of the surface atoms are changed compared to those in the bulk: growth of atomic vibration amplitude, decrease of effective Debye

92

ATTENUATED TOTAL INTERNAL REFLECTION

temperature, and so on. Reconstruction of the upper atomic planes caused by the tendency to reduce the free surface energy, and the phenomenon of a surface phase transition in the absence of one in the bulk (see Atomically clean surface) are typical for a number of crystal surfaces. The screening of the Coulomb interaction of adsorbate atoms by charge carriers in a nearby-surface space charge region can appreciably modify the atom–surface interaction. ATTENUATED TOTAL INTERNAL REFLECTION, ATR method

Technique for studying optical properties of solids (see Optics of solids), based on the phenomenon of total internal re ection of light, which occurs when a light wave penetrates from an optically denser medium 1 into medium 2 of lower optical density (n2 < n1 ). Provided that the angle of incidence ϕ exceeds the critical value ϕcrit = arcsin(n2 /n1 ) there forms a nonuniform (decaying) ﬁeld E(z) = E0 exp(−z/dpenetr ) (z is normal to the interface between the media), with an effective penetration depth dpenetr that is close to the radiation wavelength. Now, assuming that medium 2 is absorbing, the re e ctance is R = 1, which indicates the presence of attenuated total internal reﬂection. The characteristics of spectra recorded by this reﬂection (1 − R) method, and by the standard absorption method, are similar to each other. That is why attenuated total internal reﬂection is used to study strongly absorbing media, and in particular optical properties of their surfaces (e.g., perturbed unstructured layers, adsorption ﬁlms, transition layers of various origins). To enhance the contrast accumulated during repeated internal reﬂections, specially designed prisms are used that provide multiple reﬂections which effectively extend the optical path of the light wave through medium 2. The propagation of light through medium 2 may result in its polarization, so one may speak about the propagation of a volume polariton wave. From the law of the conservation of the tangential component of the wave vector kx it is possible to determine the dispersion of volume polaritons in medium 2: kx = (ω/c)[ε2 (ω)]1/2 where ε2 (ω) is the relevant dielectric constant. If medium 2 appears surface active in the respective frequency range, i.e. ε2 (ω) < 0, one may apply a modiﬁed

type of attenuated total internal reﬂection to excite surface polaritons. To that end, one introduces an air (or vacuum) gap between the prism and the material under study [Otto modiﬁcation (A. Otto, 1968)], or places the material on the base of the prism as a thin ﬁlm [Kretschmann modiﬁcation (E. Kretschmann, 1968)]. ATTO. . .

A decimal preﬁx denoting a 10−18 part of the initial unit of a given physical quantity. For example, 1 as (attoseconds) = 10−18 s (seconds). AUGER EFFECT in semiconductors (P.V. Auger, 1925)

A semiconductor analogue of the Auger effect in an atom; a double electron transition with one electron crossing to a lower level, and another one to a higher level which is often in the continuum, outside the atom. The presence of energy bands of two kinds of current carriers, and the variety of structural defects in semiconductors, leads to the wide diversity of the Auger effect. The role of this effect in nonequilibrium processes in semiconductors may be quite different: recombination, generation, impact ionization of local centers, participation in scattering processes, relaxation of the energy and momentum of charge carriers. This effect can also be a cause of the strength and of the temperature extinction of luminescence. The set of Auger effect variants is shown in Figs. (a–h). There are processes with participation of a multiply charged local center (a), singly charged local center (f, g), two singly charged local centers (b, c, d, h), and free charge carriers (e). Included among Auger processes are also all processes that are inverse to those represented in this ﬁgure. A salient feature of an Auger processes is the pronounced dependence of its probability on the distance R between the interacting carriers (∝ R −6 , corresponding to the energy of one dipole in the ﬁeld of another). In the case of an Auger interaction between free carriers, this means that the rate varies as the square of their concentration. Thus, in process (e), the hole lifetime with respect to the Auger process is proportional to the inverse square of the electron concentration, which means the dependence of the rate on R −6 . Both the theory of the Auger effect and experimental data demonstrate that the probability of this process in semiconductors is weakly

AUGER ELECTRON SPECTROSCOPY

93

Auger effect processes in semiconductors.

dependent on the temperature. The dependence of the probability on the energy exchanged between the carriers is a power function with an exponent between 2 and 5. When the distance between the electrons involved in the Auger interaction mechanism is about 10 nm in order of magnitude (corresponding to a free charge carrier concentration about 1018 cm−3 ), the cross-sections of the Auger processes can be quite large (close in a crystal unit cell size, i.e. ∼10−15 cm2 ). In this case, the Auger processes can dominate the recombination and scattering, thus determining the lifetime of the carriers, the probability of radiative and nonradiative quantum transitions, the relaxation times of energy and momentum, and other parameters of the material. AUGER ELECTRON SPECTROSCOPY

A method of analysis of the elemental and phase composition of surface layers of solids, based on the eld ionization of atoms excited by a beam of primary electrons with energies 1 to 10 keV. The sensitivity of the method is 1010 –1012 atom/cm2 , and the depth of the analyzed layer is 0.5 to 2.5 nm. The mechanism for the emergence of Auger electrons is a complicated multistage process that includes the ionization of an inner atomic level x, the ﬁlling of the produced vacancy by an electron from a higher atomic level y, the nonradiative transfer of the released excess energy to an electron

at level z, and the emission of the Auger electrons. The identiﬁcation of chemical elements is based on comparison of calculated and experimentally found values of Auger electron energy Exy = Ex − Ey − Ez + U eff . Here, Ex , Ey , and Ez are, respectively, the binding energies of electrons at x, y, and z levels (generally designated by X-ray terms) of the neutral atom participating in the Auger process; U eff is a factor to allow for the presence of two vacancies in atomic shells. Auger lines of different elements are well resolved. The change in the electron density at an atom results in a shift of the Auger line, the magnitude and sign of the shift being characteristic of the atom’s chemical state. Analysis of the width and shape of the Auger lines, whose formation is participated in by valence band electrons, yields information on the band structure of a solid. The total Auger electron current is proportional to the number of vacancies at atomic levels formed per unit time within the thickness of the region of the exit from the surface. This circumstance underlies the application of Auger electron spectroscopy to the quantitative analysis of solids. In the scanning mode of the electron beam deﬂection, Auger electron spectroscopy is used for studying the planar distribution of chemical elements with a spatial resolution of a few tens of nanometers. In combination with ion etching, it is applicable for determining the depth proﬁles of element distributions.

94

AUGER ION SPECTROSCOPY

AUGER ION SPECTROSCOPY

Determination of the elemental and chemical composition, the structure, and the state of a solid and its surface from Auger electron spectra (see Auger electron spectroscopy) excited by ion bombardment. An important feature which distinguishes Auger ion spectroscopy from Auger electron spectroscopy is its selectivity, i.e. Auger peaks of a particular kind speciﬁc for a given solid are typically observed in Auger spectra excited by ion bombardment. In addition, these peaks appear only under bombardment by certain ions. In contrast to the electron bombardment case, the character of ion-stimulated spectra is determined by characteristics of the ionization process in the inner shells, and the emission of Auger electrons at atomic collisions. In particular, the ion Auger spectra have a great number of satellites, and represent quasi-molecular spectra with a typical continuous background. Yet many of Auger peaks are narrower, since they are emitted by free atoms dislodged from the solid. Furthermore, the recoil atoms that emerge under ion bombardment and emit the Auger electrons are very fast moving, and induce an extra “Doppler” broadening (see Doppler effect). Under ion bombardment of monocrystals, one can observe both azimuthal and polar orientation effects in the Auger spectra, which are related to the crystal structure of the surface. Also classiﬁed as Auger ion spectroscopy is ion-neutralization spectroscopy that deals with the analysis of the spectrum of secondary electrons emitted during the Auger neutralization of slow positive ions (including multiply charged ones) at the solid surface. Auger ion spectroscopy is a convenient method for diagnostics of the solid surface, and is effective when one has to detect atoms of a certain element or a group of elements on the surface, or during a layer-by-layer analysis of a thin layer. This is particularly convenient in devices where ion beams are used for implantation, etching, spraying, epitaxy, etc. AUGER NEUTRALIZATION

The process whereby an ion near a solid surface traps an electron (or several electrons in the case of multiply charged ions), with subsequent transfer of the resulting energy of neutralization to another (or other) electron(s) in the solid by

means of the Auger process (see Auger effect). A condition for Auger neutralization is that the ionization potential of the ion Vi must exceed the work function of the solid ϕ (Vi > ϕ), and for electron potential emission we require Vi > 2ϕ. The Auger neutralization rate W depends on the scattering of ions to the surface S in accordance with W = A exp(−S/a) where A ∼ 1016 s−1 , a ≈ 0.2 nm. A consequence of intensive Auger neutralization is a low (≈1%) degree of ionization of atoms with high ionization potentials, e.g., inert gases reﬂected from a metal surface. Auger neutralization underlies the ion-neutralization spectroscopy of a solid surface that allows one to determine the electron density in the conduction band, the position of the Fermi level, and other characteristics of the electronic structure of a solid surface. The Auger neutralization of multiply charged ions proceeds stepwise, as a series of successive acts of Auger neutralization and Auger relaxation in the system of levels of ions with decreasing charge, with a mean step of about 25– 30 eV. As a result of the neutralization, the number of emitted Auger electrons is proportional to the resultant energy of the ion neutralization, and can be as high as a few tens of electron volts. On the surface of nonmetals this effect leads to the accumulation of a positive charge (considerably larger than the initial charge) in a microscopic region, and could possibly lead to a Coulomb explosion. This causes sputtering of the solid, and represents a mechanism for metal surface erosion under action of slow multiply charged ions. Auger neutralization of multiply charged ions on the metal surface can serve for their identiﬁcation on the background of singly charged ions due to stimulated electron emission. AUGER RELAXATION Nonradiative relaxation of an excited atom near a solid surface, an analog of the Penning effect in

gases. During Auger relaxation, the excitation energy is transferred by the Auger process to an electron of the solid, which can be emitted outward. Along with Auger neutralization, Auger relaxation is a mechanism of potential emission of electrons. This relaxation is possible for both metastable excited atoms coming to the surface, and ions that trap electrons from the solid at excited levels. The

AUTOIONIZATION

Auger relaxation time is 10−14 to 10−15 s, which is six orders of magnitude less than the time of radiative relaxation. This circumstance suppresses strongly the radiation of the excited atoms near the metal surface. On the surface of nonmetals or metals covered by adsorbed layers, the rate of the Auger relaxation can be slightly smaller. AUGMENTED PLANE WAVES METHOD, APW method (J.C. Slater, 1937) One of the main band structure computation methods. It considers crystal potentials in the form of a muf n-tin potential (MT potential) and is based

on the variational principle. Its basis functions are the APWs. Outside the MT-sphere an APW is a plane wave, ei(k+G)r (G is a reciprocal lattice vector). Inside the MT-sphere the APW method employs a linear combination of solutions of the Schrödinger equation in a spherically symmetric potential. The coefﬁcients for that combination are selected to satisfy the continuity condition for APWs at the MT-sphere boundary. The amount of computations needed follows from the necessity of solving a nonlinear secular equation of high order. The order of the equation, i.e. the number of APWs, is usually quite large, from several dozen for the simplest lattices to several hundred for polyatomic structures. For the linearized APW method, see Linear methods of band structure computation. AUSTENITE (named after W. Roberts of Austen) A high-temperature gamma phase that is a solid solution of carbon (or nickel, manganese, ni-

trogen) in γ -iron with a face-centered cubic lattice (see Face-centered lattice). Alloying with these elements stabilizes γ -iron. Alloys in which the γ -state is present at room temperature are called austenite alloys. They are easily deformable and possess high corrosion resistance. Carbonaceous austenite is stable under cooling to 725 ◦ C; at lower temperatures, a phase transition occurs which can proceed either in a diffusion or a nondiffusion manner, depending on the cooling rate or the isothermal exposure. At cooling rates of a few tens of a deg/s or at isothermal exposure in the temperature range 450–723 ◦ C, the austenite decomposes into a ferrite–cementite mixture (see Cementite) and forms structures of a

95

pearlite class (pearlite, sorbite, troostite) that differ in the degree of dispersion of cementite plates. At temperatures below 450 ◦ C, when the diffusion rate of iron and alloying elements is insufﬁcient, austenite transforms into bainite; the transformation needs only the diffusion of carbon. At lower temperatures and at a cooling rate greater than 100 deg/s, austenite transforms into martensite in a diffusionless manner (see Martensitic transformation). When overheated above the critical point, perlite transforms into austenite at a varying rate; however, the newly formed austenite is heterogeneous even within a single grain volume. To obtain a homogeneous austenite, it is necessary to operate at a temperature above the completion of the perlite–austenite transformation, which produces homogenization. The rate of the homogenization is largely determined by the initial structure of the steel. The trends of the processes of decomposition (see Alloy decomposition) and formation of austenite underlie the processes taking place during the heat treatment of steel, with the treatment providing the required combination of strength and durability properties of steel. AUTOEPITAXY, homoepitaxy

The oriented and ordered build-up of a material on a monocrystal surface of the same material. Autoepitaxy is observed in the deposition of material from liquid solutions or melts, by chemical reactions at crystallization from the gas (vapor) phase, and at condensation from vapors in vacuo. In autoepitaxy the crystal lattice of the building-up phase is oriented relative to the lattice of the substrate monocrystal. Important inﬂuences on autoepitaxy are the chemical purity and the distribution of defects on the monocrystal surface, the chemical composition of the environment, the temperature, the goodness of the vacuum chamber, and the chemical composition of the residual atmosphere. The phenomenon of autoepitaxy is used to prepare thin lms of germanium, silicon, gallium arsenide and other semiconductors on monocrystal substrates of the same materials (see also Epitaxy). AUTOIONIC MICROSCOPY The same as Field ion microscopy. AUTOIONIZATION The same as Field ionization.

96

AUTOPHOTOELECTRONIC EMISSION

AUTOPHOTOELECTRONIC EMISSION

AUTOWAVES

Electronic emission by a conducting body being irradiated by light in the presence of a strong external electric ﬁeld (of the order of 109 V/m). The mechanism of autophotoelectronic emission is the eld electron emission excited by light. This emission appears most prominently in p-type semiconductors at low temperatures. The light excites the electrons from the valence band to the conduction band, with the long wavelength (red) limit of photosensitivity determined by the width of the band gap. The external electric ﬁeld penetrates deeply inside the cathode and facilitates the transport of electrons to the surface and their escape into the vacuum. The quantum yield can reach 0.5–0.8. Autophotoelectronic emission is used in converters of images in infrared rays to visible images. The cathodes in such converters are multitip (up to 106 tips/cm2 ) matrix systems of p-type semiconductors (silicon, germanium, and others).

Nonlinear waves in an active medium, in which the energy dissipation is compensated by an applied external source; the analog of the selfoscillations for distributed oscillatory systems. As distinct from auto-oscillations, when the system oscillates as a whole, in autowave processes the excitation is transferred between neighboring elements of the medium (the term autowaves was introduced by R.V. Khokhlov). There is a great variety of autowave process types in nonequilibrium systems. They are described by systems of non-linear differential equations; a typical form of the equation for the variables Ui , e.g., temperature, particle concentration (quasiparticles in solids), electric ﬁeld, etc., is

AUTORADIOGRAPHY, radioautography

Analysis of the radioactivity distribution in a material by means of autoradiograms which are photographic images produced by radioactive emission. Autoradiography is based on the ability of some substances (typically, silver bromide) to undergo chemical transformations under the action of light, X-rays, gamma rays, and charged particles. Using contact contrast analysis, the emission intensity and the radioactive isotope distribution in the material are determined by the extent, density, and distribution of the blackening of the various regions of the autoradiograms. To obtain and analyze the autoradiogram, a sample containing the radioactive isotope is brought into contact with the photoemulsion and kept in position there for some time (up to several days), depending on the emission type and intensity. Then the autoradiogram is developed and analyzed by means of an optical or electron microscope. In the latter case, the object under study is a carbon replica with emulsion deposited on its surface. Autoradiography is used in the tracer analysis method for studying the distribution of doping elements and impurities in various materials, for measuring their mobilities, etc.

∂Ui = Di ∇ 2 Ui + Fi (U ), ∂t where t is the time, and ∇ 2 is the Laplacian. The ﬁrst term describes the evolution of Ui relative to the spatial spreading of this nonuniformly distributed variable (if Ui is the particle concentration, then Di is the diffusion coef cient, if Ui is the temperature, then Di is the thermal conductivity coefcie nt, etc.). The functions Fi (U ), where U is a totality of the all the individual Ui , describe the non-linearity of the medium, and the interaction between different components of U . These functions include the permanent energy source, which covers the energy dissipation expenditure. There are also more complicated sets of equations describing autowave processes. Self-organization is possible (see Synergism) in autowave media, i.e. the spontaneous regularization of both the temporal evolution of the system (rise of periodic or more complex oscillations) and the spatial distribution of its characteristics (emergence of dissipative structures). However, complete randomization of autowaves often occurs. Autowave processes are widespread in nature, occurring in many biological systems, and in physical and chemical transformations (e.g., combustion and other reactions, gas discharges). In solids, autowave modes are often realized in the excitation of the electron subsystem: in semiconductors by an electric ﬁeld, by heating, by the injection of charge carriers (thermoelectric domains, Gunn effect, recombination waves, electron–hole

AZBEL–KANER RESONANCE

drops, etc.); in phase transitions, e.g., a metal– semiconductor transition, in ferroelectric phase transitions, in active non-linear optical solid media (lasers, real-time holography), etc. The autowave processes in solids are characterized by a variety of spatial–temporal scales (diffusion length 105 –10−7 cm, frequency 10−2 –1010 Hz), and mechanisms of the excitation transfer (ﬂuxes of electrons and holes, excitons, magnons, phonons, photons). Applications of autowaves are extensive, including, for example, optical, radio-, and UHF ampliﬁers and generators; generation of ultra- and hypersound; recording and processing of information; image recognition; processes (propagation of nerve impulses and regimes of cardiac muscle operation), etc. AVALANCHE OF PHONONS See Phonon avalanche.

97

AVOGADRO NUMBER (A. Avogadro, 1811) The number of molecules (atoms, ions) in one mole, identical for any substance in any state of matter; NA = 6.02214·1023 mole−1 . One mole

(gram-molecule) is the mass of a substance in grams, numerically equal to its atomic or molecular weight. The unit of molecular weight is 1/12 of the mass of the carbon isotope 12 C. In the SI system, the mole is accepted as the unit of the quantity of a substance. AXIAL SYMMETRY

The symmetry of a body, which comes into coincidence with itself when rotated through an arbitrary angle about some axis. Such a rotation symmetry axis (∞) pertains to cones and cylinders with the limiting symmetry groups ∞, ∞2, ∞m, ∞ , ∞ m corresponding to them. m m AZBEL–KANER RESONANCE The same as Cyclotron resonance in metals.

This Page Intentionally Left Blank

Bb named after E. Bain. In carbon steels, bainite forms during the isothermal hardening process as a result of decomposition of the austenite (see Alloy decomposition) in the temperature range 250–450 ◦ C. In some alloyed steels (see Alloying), bainite can appear during cooling in air. The conditions of decomposition (mainly, thermal conditions) of the overcooled austenite,determine the formation of higher bainite or lower bainite with speciﬁc morphologic and crystalline features. The transition between them occurs at 350 ◦ C. The bainite structure allows one to process steels that have high static, dynamic and cyclic strength as well as wear resistance and elasticity.

BACKSCATTERING of high-energy particles Occurs under bombardment of a solid surface,

and results from collisions of incoming particles with atoms of the target. In this case the direction of the normal component of the particle momentum may change, which causes some of the particles that have penetrated into the target to escape back through the surface under bombardment. Contributions to backscattering come from both single scattering through large angles, and from multiple scattering. The energy and angular distribution of the scattered particles carry information about the masses of the target atoms; it is the collisions with these atoms in the nearsurface region that determine the energy loss by the incident particles. This effect is used for the analysis of the elemental composition of materials, including their impurities. Ions with energy E 1 keV are almost completely backscattered from most solids. At E 10 keV, a signiﬁcant number of ions penetrates into the target, thus reducing the efﬁciency of the backscattering, especially for heavy ions. The energy of the escaped atoms decreases with increasing depth z where the reversal in direction occurrs, thus allowing an estimate of z. The efﬁciency of the backscattering method for determining the content of defects in crystals (especially impurity and intrinsic interstitial atoms) grows signiﬁcantly for irradiation in the channeling regime. Here, one can determine the positions of interstitial atoms in the channels of a monocrystal target with a good accuracy, and detect the disordering of crystal lattices at a depth of several micrometers from a surface that is irradiated with ions.

BALLISTIC AFTEREFFECT

An inertia effect occurring when a magnetic bubble domain is displaced under the action of a pulse of a nonuniform magnetizing ﬁeld, and continues its motion at the initial speed after the pulse termination. The path covered can be much greater than the domain displacement during the pulse action. The ballistic aftereffect is observable only when the magnetizing ﬁeld gradient along the domain diameter exceeds a certain critical value. The cause of the ballistic aftereffect is as follows: in the overcritical regime, there appears a great number of horizontal and vertical Bloch lines in the magnetic domain wall of the magnetic bubble domain; these lines are dynamically stabilized and accumulate considerable mechanical momentum. After turning off the nonuniform magnetic ﬁeld, the magnetization distribution in the domain wall becomes unstable, and the process of “untwisting” of the Bloch lines begins. The decrease of accumulated mechanical momentum is compensated for by the motion of the domain as a whole. The magnetic bubble domain eventually comes to a stop due to viscous friction forces (see Domain wall drag).

BAINITE, acicular troostite

A structural component of steel, a highly disperse mixture of ferrite and iron carbide. It was 99

100

BALLISTIC PHONONS

BALLISTIC PHONONS

Nonequilibrium acoustic phonons propagating unhindered in crystalline solids, usually in straight line paths without scattering by lattice defects, free current carriers and impurity atoms, and also free of phonon–phonon scattering at low temperatures. A typical distance that phonons of frequency nm (or equivalently κ > 0); where g is the density of electron states at the Fermi surface. The drawbacks of the Stoner model have not yet been completely overcome. One of them is the disregard of the Bloch factor in the wave function of the electrons, the factor having the period of the crystal lattice, which precludes the quantitative treatment of the situation ζ > ε, and thus restricts quantitative results to the case of so-called weak band ferromagnets (κ 1). Another drawback involves the molecular ﬁeld approach that is inapplicable in the neighborhood of the Curie point T C (near point T = T C , B = 0 in the (T , B) plane). Following from Eqs. (1) is the so-called Wohlfarth isotherm (E.P. Wohlfarth, 1968), which is the

102

BAND STRUCTURE

dependence of the magnetization of a band ferromagnet on B and T : m(B, T ) 3 m(B, T ) T2 2χ B − 1− 2 = 0 , m0 m0 m0 TC (2) where m0 ≡ m(0, 0), and χ0 is the longitudinal (in B) static magnetic susceptibility at T = 0. Eq. (2) is quantitatively valid for weak band ferromagnets, e.g., ZrZn2 , ScIn, Ni3 Ga, and a number of Fe–Ni–Mn alloys. The quadratic dependence of the spontaneous magnetization on the temperature, which follows from Eq. (2), viz. m20 − m2 (T ) ∝ T 2 , was also experimentally observed in strong band ferromagnets (3d-metals and alloys). The theory of magnons in band ferromagnets is based on the work of A.A. Abrikosov and I.E. Dzyaloshinskii. The temperature dependence of the magnon spectrum in band ferromagnets was studied by V.P. Silin and others. If the Stoner criterion (1) is not met then the metal is paramagnetic. If, however, |κ| 1, then strong band paramagnetism occurs (for band antiferromagnetism see Antiferromagnetic metals, Spin density wave). BAND STRUCTURE

This is the energy spectrum (plots of average energy E versus wave number k) of singleelectron states represented in the form of a dispersion law of electrons Ekλ , where k is the quasiwave vector, λ is a quantum number called the band index or band number. Occasionally, electronic wave functions are also included in this definition. The band structure is a key notion of the band theory of solids. See also Band structrure computation methods. BAND STRUCTURE COMPUTATION See Linear methods of band structure computation. BAND STRUCTURE COMPUTATION METHODS

Procedures and algorithms for solving the single-particle Schrödinger equation in a periodic potential by using modern computers. The construction of a crystalline potential, self-consistent in the sense of density functional theory, is an

important part of band structure computation. Pseudopotential methods generally incorporate a weak pseudopotential; and full-electron methods place no restrictions on the potential strength. Early band structure computation methods had been developed even before high-speed computers were available. These were the augmented plane waves method (APW), Korringa–Kohn–Rostoker method (KKR), orthogonalized plane waves method (pseudopotential method, version I), and tight binding method. The APW and KKR methods are designed for a potential of a special form. The further development of band structure computation methods was chieﬂy determined by the emergence of linear methods of band structure computation, e.g., linear combination of atomic orbitals (LCAO), linear APW, etc., and generalizations of the methods of the APW and KKR families to potentials of arbitrary form. Standing apart are methods related to the tight binding approach, viz. the linear combination of atomic orbitals method (Gaussian orbitals and Slater orbitals). One can notice their connection to the methods of the KKR theory. The time required for computing the band structure is determined, mainly, by the number of atoms in a unit cell. In most of the methods the computational time grows approximately proportional to the cube of this number. BAND STRUCTURE, SURFACE See Surface band structure. BAND THEORY of solids

A theory describing a crystalline metal or solid as a system of noninteracting electrons, moving in a periodic potential. The potential is assumed to arise from nuclei or positive ions screened by electrons. The effects of mutual interactions are considered to be included in the effective potential. The Bragg scattering of electrons in the crystal potential results in a complicated dependence of electron energies on quasi-momenta (so-called band structure), with the appearance of band gaps, i.e. energy gaps where the electrons have no allowed states. In the ground state, at zero temperature, all electron states with energies lower than the chemical potential (referred to in band theory as the Fermi energy E F , or Fermi level) are occupied,

BAND THEORY

103

Energy bands of (a) the insulator crystalline xenon, (b) the semiconductor silicon, (c) the transition metal molybdenum, and (d) the nearly free electron metal sodium.

and those with higher energies than the chemical potential are empty. In semiconductors and insulators the chemical potential lies within the gap, so there are no allowed states with the energy E F itself. There are such states in a metal, and they form a surface in k -space, called the Fermi surface. An important parameter of the electronic spectrum is the density of electron states, which indicates the number of allowed states per unit energy at a given energy. The density of states at the Fermi level is of special importance. The main task in band theory is to solve the one-electron Schrödinger equation in a crystal potential with translational symmetry. The latter imposes certain constraints on a solution ψk with quasi-momentum k: ψk (r + R) = ψk (r)eikR , where R is a lattice translation period (Bloch theorem). Such solutions are called Bloch wave functions. The requirements of crystal symmetry also impose other constraints on the wave functions and the electron energy spectrum, and these are often used to simplify the solution of the

Schrödinger equation. However, in the vicinity of nuclei the inﬂuence of crystal symmetry is not pronounced, and the potential is close to an atomic one. Hence, it is possible to speak about electronic states (or bands) of predominantly s-, p- or d-type character, similar to the classiﬁcation of states according to the atomic angular momentum. Band theory permits the classiﬁcation of solids according to the qualitative features of their band structure. In insulators the allowed bands do not overlap, and some are completely full (valence bands), while the remainder are empty (conduction bands). Semiconductors differ from insulators only by their small (fraction of an electronvolt) width of the forbidden gap. In metals the Fermi level lies within the allowed band, or more commonly, the allowed bands overlap one another. In semimetals, the overlap of these bands also occurs, but to a lesser extent. There is also a separate class of gapless semiconductors, distinguished by the width of the forbidden gap becoming zero at one or several points of the Brillouin zone.

104

BAND THEORY RELATIVISTIC EFFECTS

Quantitative band theory is based on the numerical solution of the Schrödinger equation in a crystal. Initially used for this purpose were the nearly-free electron approximation and the tight binding method, which are valid within the limits, respectively, of a weak crystal potential, and of a potential consisting of isolated wells separated by high barriers. Later the pseudopotential method was developed, which expanded the applicability of the method of nearly-free electrons. More widely used are non-pseudopotential methods, capable of dealing with more generalized types of crystal potentials. With the appearance of density functional theory, a formal basis emerged for the transformation in the effective potential from a system of strongly interacting electrons to that of noninteracting particles, i.e. to band theory proper. Linear methods of band structure computation have been elaborated, which permit solving the Schrödinger equation in a crystal 2 to 3 orders of magnitude faster than by using classical methods of computation. Typical examples of band structures are shown in Fig. (see previous page): (a) an insulator (crystalline Xe) with a narrow valence band, a wide gap, and bands well described by the tight binding method; (b) a semiconductor (Si) with its indirect gap width small compared to that of the valence band; (c) a transition metal (Mo) with valence electrons comprising the group of bands formed predominantly by s- and d-electrons; where the Fermi level lies inside the d-band with a high density of states; and (d) a simple metal (Na) with s-electrons forming an almost parabolic energy band with a low density of states, in accordance with the model of nearly free electrons, where X, Γ , L, N , and P are symmetry points of the Brillouin zone. BAND THEORY RELATIVISTIC EFFECTS See Relativistic effects in band theory of metals. BAND-TO-BAND TUNNELING See Interband tunneling. BARDEEN BARRIER (J. Bardeen)

A potential barrier which emerges at the boundary between two bodies in contact (e.g., two solids, a solid and a liquid or gas) in the presence of a signiﬁcant concentration of surface electron states at

the interface. In the limit of high concentrations, the Bardeen barrier height does not depend on the contact potential difference due to screening of the Coulomb interaction by the charges in the surface electron state. In practice, the Fermi level of a Bardeen barrier is ﬁxed at the surface (at the interface). In most cases, this term is used with respect to contacts between a semiconductor and a metal (called a Schottky barrier), an insulator, or another semiconductor. BARDEEN–COOPER–SCHRIEFFER THEORY, BCS theory (J. Bardeen, L. Cooper, J. Schrieffer, 1957)

The ﬁrst and the currently accepted microscopic theory of superconductivity based on the presence of so-called Cooper pairs in a superconductor at low temperatures T < T c (where T c is the critical temperature). The Cooper pairs consist of electrons with antiparallel momenta and spins (see Cooper effect) that form as a result of their attraction via the electron–phonon interaction. The starting point of the theory is the model Hamiltonian + 2εk ckσ ckσ + Vkk bk+ bk , (1) HBCS = k,k

k

where εk is the initial energy of the conduction + and ckσ are electrons with momentum k, ckσ the creation and annihilation operators of electrons, respectively, bk+ and bk are the same for the Cooper pairs (see Second quantization), and Vkk are the matrix elements of the effective electron– electron interaction. The minimization of the energy of the ground state of the electron subsystem of the superconductor yields the following expression for the quasi-particle spectrum through the use of the variational method within the BCS framework: 1/2 , (2) Ek = (εk − μ)2 + Δ2k where μ is the chemical potential (Fermi level) of the degenerate electrons in the metal, and Δk is the energy gap determined by the following nonlinear equation: Δ Δ (3) Vkk k tanh k . Δk = − 2E 2k BT k k

A nontrivial solution of Eq. (3) Δk = 0 exists only for the condition Vkk ≡ V < 0, i.e. so in a cer-

BARIUM TITANATE

tain range of energy (momentum) of the Fermi surface of a metal, the effective attraction due to the electron–photon interaction exceeds the screened Coulomb repulsion (see Electric charge screening). In the weak coupling limit Eq. (3) yields the exponential BCS formula for the gap Δ at T = 0: 1 , (4) Δ = 2ωD exp − N(0)V (where ωD is the Debye phonon frequency, and N(0) is the electron density of states on the Fermi surface in a normal metal), and for the critical temperature T c of the transition to the superconducting state we have: 2eγ 1 , (5) Tc = ΘD exp − π N(0)V where ΘD = ωD /k B is the Debye temperature. Eqs. (4) and (5) give the BCS relationship k B T c = eγ Δ0 /π = 0.567Δ0 , where k B is the Boltzmann constant and γ = 0.577. . . is the Euler–Mascheroni constant. The BCS relationship is valid solely for superconductors with weak coupling, whereas for strongly-coupled superconductors k B T c < γ Δ(0)/π . The latter is due to the effects of the retardation of the electron–phonon interaction, which cause the gap Δ to depend on the energy of the quasi-particles and, hence, the value of Δ at T = 0 increases compared to the value πk B T c /eγ . The BCS theory has explained the principal physical properties of superconductors in terms of the presence of the energy gap in the quasi-particle spectrum. This includes magnetic vortices, ﬂux quantization, the exponential dependence of the electron speci c heat on the temperature and its jump in value at the phase transition point T = T c ; the temperature dependence of the thermodynamic critical magnetic eld; the features of ultrasound attenuation; relaxation of nuclear spins, and the absorption of electromagnetic waves in superconductors; the current–voltage characteristics of the superconducting tunnel junctions, and so on. The originators of the BCS theory received the Nobel prize in 1972. BARIUM, Ba

A chemical element of Group II of the periodic system with atomic number 56 and atomic mass 137.33. It consists of a mixture of seven sta-

105

ble isotopes, with 138 Ba predominating (71.66%). The electronic conﬁguration of the outer shell is 6s 2 . Successive ionization energies are 5.21 and 10.00 eV. Atomic radius is 0.221; ionic radius of Ba2+ is 0.134 nm. Oxidation state is +2. Electronegativity is ≈0.94. In a free form barium is a silvery-white soft metal. It has a body-centered cubic lattice with parameter a = 0.5019 nm at ¯ (O 9 ). room temperature; Space group is I m3m h 3 Density is 3.76 g/cm ; T melting = 998 K; heat of melting is 7.66 kJ/mole; heat of sublimation is 205 kJ/mole; T boiling = 1912 K; heat of evaporation is 175 kJ/mole; speciﬁc heat is 284.7 kJ·kg−1 ·K−1 ; Debye temperature is 110 K; coefﬁcient of linear thermal expansion is ≈19.5·10−6 K−1 (at 273 to 373 K); adiabatic bulk modulus is 9.575 GPa; Young’s modulus is 15.57 GPa; rigidity is 6.33 GPa; Poisson ratio is 0.229 (at 293 K); Brinell hardness 0.042 GPa; Mohs hardness is 2; ion-plasma frequency is 4.52 THz, Sommerfeld linear electronic speciﬁc heat coefﬁcient γ is 2.72 mJ·mole−1 ·K−2 ; electric resistivity is 357 n·m (at 293 K); temperature coefﬁcient of the electrical resistance is 0.00649 K−1 ; work function of a polycrystal is 2.49 eV; molar magnetic susceptibility is 20.4·10−6 cgs units; nuclear magnetic moment of 137 Ba is 0.931 nuclear magnetons. Barium is used in alloys with lead, aluminum, and magnesium. Barium and its compounds are added to the materials intended for protection against radioactive and X-ray radiation. BARIUM TITANATE, BaTiO3

A colorless solid substance; T melting ∼ 1618 K; it has the structure of perovskite (tetragonal crystal lattice with lattice constants a = 0.3992 nm, c = 0.4036 nm); density is 6.08 g/cm3 . Each titanium is surrounded by a somewhat distorted octahedron of oxygens. Chemically it is very resistant: it does not change in air or react with water, diluted acids or alkali; it dissolves in hot strong sulfuric acid. It is an insulator with a very high dielectric constant (1000 at 20 ◦ C), and one of the most important ferroelectrics with a high piezoelectric modulus (see Piezoelectricity) and speciﬁc optical properties. It is obtained by caking and melting together of titanium dioxide with barium oxide, hydroxide or carbonate, or

106

BARKHAUSEN EFFECT

by heating up to 800 to 1200 ◦ C of mixture obtained by common deposition of carbonates or oxalates from solutions. It is used in the form of monocrystals and solid solutions for manufacturing of capacitors, piezoelectric cells, pyroelectric collectors of radioactive energy, etc. BARKHAUSEN EFFECT (H.G. Barkhausen, 1919) A jump-like change of magnetization M in

magnetically ordered materials under continuous variation of external conditions (e.g., applied magnetic ﬁeld B). Barkhausen discovered that clicks could be heard in a telephone supplied by an electron ampliﬁer and connected with a coil containing a ferromagnetic sample during very slow (quasi-static) magnetizing of the latter. The main cause of a Barkhausen effect is the various inhomogeneities of the crystalline structure of a ferromagnet (inclusions, residual stresses, dislocations, grain boundaries, the heterogeneity of the composition, and other defects in the crystals). When moving in the magnetic ﬁeld, the magnetic domain walls attach to these inhomogeneities until the increasing ﬁeld reaches a certain (critical) value. Then the domain wall is released (Barkhausen jump), so that its motion turns out to be jump-like, in contrast to a smooth movement in a perfect crystal. These jump-like changes are irreversible. Another mechanism of the Barkhausen effect is possible: the nucleation of new phase centers with their subsequent growth. The Barkhausen effect is best observable in soft magnetical materials at the steepest part of the magnetization curve (of stepped shape in that region, see Fig.). This effect

is highly sensitive to various external factors and structural changes in the sample. The connection of the Barkhausen effect with the magnetic domain structure, the main elements and the shape of the hysteresis loop, allows it to be used as a method of investigation of the domain structure of ferromagnets. By analogy with ferromagnets, the appearance of repolarization jumps in ferroelectric crystals under variation of an applied electric ﬁeld is also referred to as a Barkhausen effect. BARKHAUSEN NOISE

Irregular sequences of jumps in the the magnetic moment of a ferromagnetic sample placed in a periodically varying magnetic ﬁeld (see Barkhausen effect). The component is due to ﬂuctuations of speciﬁc parameters of Barkhausen jumps (the shape and duration, the critical ﬁeld, the magnetic moment varying at the jump, the number of jumps in a given range). Studies of Barkhausen noise yield substantial information on complicated phenomena involving the rearrangement of the magnetic domain structure in ferromagnets. BARNETT EFFECT (S. Barnett, 1909) Magnetizing of ferromagnets under a change in

their mechanical moment. Barnett conﬁrmed Ampère’s hypothesis that magnetism can arise from rotational motion of charges in a material (molecular current hypothesis). In a body with no atomic magnetic structure, the intrinsic magnetic moment is proportional to the angular velocity and oriented along the rotation axis. In some cases, the Barnett effect allows one to determine the gyromagnetic ratio or Landé g -factor of atoms of some materials. In particular, this ratio for Fe, Co, Ni and their alloys corresponds to the electron magnetic moment and indicates that ferromagnetism is mainly due to the electron spin. The Barnett effect, along with the converse Einstein–de Haas effect, are called magnetomechanical phenomena. Magnetic resonance methods are much more precise for determining g-factors. BARODIFFUSIONAL EFFECT An effect of hydrostatic pressure on the diffusion healing of defects, or the retardation of pore

Barkhausen effect.

growth (at low pressures), and on the decrease of

BARRIER INJECTION TRANSIT TIME DIODE

the diffusion coef cient in crystals (at high pressures). At low pressures, barodiffusional effects are caused by the inﬂuence of pressure on the equilibrium between the pore and the vacancy subsystem (see Vacancy) taking into account oversaturation Δ = cv − cv0 in a crystal (where cv and cv0 are the actual and equilibrium concentrations of vacancies, respectively). Under the characteristic pressure Pk = 2α/R0k (where α is the surface tension, R0k is the critical radius of a viable pore embryo in the absence of pressure), the nucleation and the growth of pores are forbidden. At R0k = 10−5 cm, Pk ≈ 102 atm. Such pressure has a signiﬁcant effect on the kinetics of the diffusional coalescence of the pore ensemble due to the transformation of some of the growing pores into dissolving ones. Under high pressures, the barodiffusional effect is caused by the decrease of cv and by the increase of the energy outlay for an elementary migration event with growing pressure. There is an exponential diffusion coefﬁcient dependence ω P , DP = DP 0 exp − A kBT where ωA = ωv + ωm is the activation volume, ωv < ω is the vacancy volume dependent on the extent of relaxation of the atoms surrounding the vacancy, ω is the atomic volume, ωm is the volume of the activated complex at a crossing point between two neighboring positions. It follows from the dependence DP (P ) that at a characteristic pressure P ∗ = k B T /ωA the value of DP reduces e times. For metals, P ∗ ≈ 104 atm. BARRETT FORMULA (J.H. Barrett)

An expression describing the temperature dependence of the dielectric constant of ferroelectrics in the paraelectric phase in a temperature (T ) range that includes the quantum region: ε(T ) − ε∞ −1 Ω0 Ω0 =C , −Tc coth 2k B 2k B T where Ω0 is the frequency of zero-point vibrations, T c is the “high-temperature” value of the Curie–Weiss temperature. At T > Ω0 /k B , the

107

Barrett formula transforms into the classical expression since ε(T ) satisﬁes the Curie–Weiss law. The system behavior at T Ω0 /k B depends on the ratio of T c and Ω0 /(2k B ). If T c > Ω0 /(2k B ), the system has a low-temperature phase transition at T = T cL < T c . There is no ferroelectric phase transition, if T c < Ω0 /(2k B ), in this case the crystal is a virtual ferroelectric. The Barrett formula is used to explain the observed low-temperature values ε(T ) in SrTiO3 and KTaO3 , but is only valid when the soft mode frequency is high relative to acoustical frequencies. In the general case, taking into account the interaction of optical vibrations and acoustic vibrations results in a characteristic modiﬁcation of the Barrett formula in a low-temperature range. BARRIER See Bardeen barrier, Lomer–Cottrell barrier, Potential barrier, Schottky barrier, Local barriers, Surface barrier, Surface barrier structures. BARRIER CAPACITANCE, junction capacitance

Electric capacitance caused by the existence of a potential barrier in a semiconductor junction, in a heterojunction, at a metal–semiconductor junction, and so on. Such a system possesses a high-ohmic layer that is depleted of current carriers and situated between high-conduction layers, i.e. is similar to a capacitor. The electric charge in the depletion layer is concentrated at local electronic levels. The barrier capacitance value is determined by the thickness of the depletion layer and the dielectric constant of the crystal. A layer with an increased current carrier concentration also has a barrier capacitance, e.g., an accumulation layer in the metal– insulator–semiconductor structure. BARRIER INJECTION TRANSIT TIME DIODE (BARRITT diode) A superhigh-frequency (SHF) semiconductor diode consisting of a semiconductor plate with contacts made of semiconductor junctions

(p+ –n–p+ , p+ –n1 –n2 –p+ , where n1 > n2 , and other structures), Schottky barriers (m–n–m structures, m is metal), or their combinations. With the bias voltage applied to the diode, one contact operates in the forward direction and the other in the reverse direction. A BARRITT diode operates in a

108

BARRITT DIODE

punch-through mode where the depletion regions of the forward- and reverse-biased contacts overlap, so that a small change of the voltage across the diode results in the current growing by several orders of magnitude. Dynamic negative resistance in the BARRITT diode arises in a frequency range ω where the phase delay of carrier transit through the depletion layer of the reversebias junction is θ = ωτ ≈ 3π/2 (τ is carrier transit time). The barrier drift time through the depletion layer of the reverse biased junction depends on the width of the depletion layer and the saturation velocity. The effect is due to the phase shift between the SHF electric ﬁeld and the conduction current. The required phase shift is caused: (i) by the phase delay of the injection of the minority charge carriers through the forward biased p–n junction, and (ii) by the ﬁnite time of the current carrier drift through the depletion layer. BARRITT diodes are used for signal generation and ampliﬁcation in the frequency range from 3 to 15 GHz. The main advantage of these diodes is a low noise level. BARRITT DIODE The same as Barrier injection transit time diode. BASAL PLANE of crystals

A plane containing equivalent crystallographic (coordinate) axes x and y. Ordinarily it is the plane that forms the bottom of the conventional unit cell, with the index (001) in tetragonal and (0001) in trigonal and hexagonal crystals (see Crystallographic system). The spatial arrangement of the faces and the sides of crystalline polyhedra is described with the help of symbols relative to these axes. The faces that intersect only one axis and possess numbers (100), (010) and (001) (see Crystallographic indices) are called basal (coordinate) faces. BASALT

An extrusive and congealed dark gray or black volcanic rock consisting mainly of plagioclase, pyroxenes and often olivine, typically with an admixture of magnetite or ilmenite. Color is dark sulfur-like to black. Basalt forms frequently have a rod-like or a “pencil”-like separation. Holocrystalline basalt is called dolerite; basalt of vitreous texture is called hyalobasalt.

The almond-shaped basalts, or mandelstones, are porous varieties. The pores (voids) are of a rounded, ellipsoidal, more rarely elongated, tubular shape and are ﬁlled with minerals, mostly, agate, chalcedony, opal, quartz, or sometimes, amethyst, zeolites, calcite, and so on. The density is 2.8–3.2 g/cm3 ; the resistance to compression in a dry state is 300–500 kg/cm2 (3–5 MPa); electric resistivity ρ = 103 –105 ·m; porosity is 7.9%, water absorption is 1.07%, and magnetic susceptibility χ = (125–15500)·106 CGS units. The basalts are used as building, electric insulation, and acid-resistant materials. BAUSCHINGER EFFECT (J. Bauschinger, 1886) A partial dehardening of single and polycrys-

talline solids observable at the change in the sign of the strain. The effect manifests itself as a reduction of some initial mechanical properties (elastic limit, yield limit, and so on) when, prior to a test, a sample was loaded in the opposite direction until an insigniﬁcant residual strain appears. The Bauschinger effect is observable both in static tests and in the course of fatigue loading (see Fatigue). At the same time, its value depends essentially on the kind of material, of the material pretreatment, and the strain conditions. Numerous attempts have been made to explain the Bauschinger effect on the basis of dislocation theory (see Dislocations); however, a satisfying agreement with the experimental data has been achieved only in individual cases. BEER–LAMBERT LAW (also called Bouguer–Lambert–Beer law, P. Bouguer, J.H. Lambert, A. Beer)

A law determining the dependence of the intensity I of a parallel monochromatic light beam on the thickness d of the absorbing matter: I = I0 e−kd ,

(1)

where I0 is the incident light intensity, k is the absorption coef cient (cm−1 or m−1 ). The latter is related to the dimensionless absorption index κ as k = 4πκ/λ, where λ is the wavelength. Eq. (1) is used to evaluate the absorptivity of a solid or liquid layer. For a dilute solid or liquid solution of concentration n, Eq. (1) takes the form: I = I0 e−χnd ,

(2)

BERYLLIUM

where χ is the molecular absorption index, cm2 . In the particle beam radiation of solids the term absorption cross-section is often employed for χ , and k is referred to as the absorption factor. Sometimes the Beer–Lambert law is expressed in terms of common logarithms (i.e. a power of 10) as I = I0 · 10−εcd ,

(3)

where c is the molar concentration, and ε is the decimal molar absorption index, also called the absorption or extinction coefﬁcient. BEILBY LAYER (G.T. Beilby, 1901) A glass-like surface layer that appears during mechanical processing (grinding, polishing, forging, punching, cutting, and so on) at the surface and over the grain boundaries of crystalline solids (metals, quartz, various minerals and chem-

ical compounds). A Beilby layer has its normal crystal structure obliterated. Long term grinding or polishing is unable to remove the layer, but rather causes its thickness to grow. A Beilby layer is removable by chemical methods. Its thickness ranges from a several to 100 or more microns. A Beilby layer along grain boundaries imparts great strength to a material, it is characterized by pronounced hardness, and speciﬁc optical, electric, and magnetic properties. A Beilby layer crystallizes under heating at a temperature between 0.4 and 0.6 that of the melting temperature. BENDING VIBRATIONS of a crystal lattice Vibrations of chains (layers) of crystal atoms

in a direction normal to the chains (layers). Bending vibrations exist in those crystals where the bonding between the chains (layers) is weak compared to that of the atoms within the chain (layer). The linear dispersion law for bending vibrations is valid only for the lowest values of the wave vector along the chain (layer). At large values of the wave vector, a quadratic dispersion law similar to that for the vibrations of strings and membranes applies. BERKELIUM, Bk An actinide element of Group III of the peri-

odic system with atomic number 97 and atomic mass 247.07.

109

There are 11 known radioactive isotopes with mass numbers 240, 242 to 251 (no stable isotopes have been discovered). Electronic conﬁguration of outer shells is 5f 7 6d 2 7s 2 . Ionization energy is 6.30 eV; atomic radius is 0.174 nm; radius of Bk3+ ion is 0.0955 nm, of Bk4+ ion is 0.0870 nm. Oxidation state is +3 (most stable in solution) and +4 (strong oxidizer). Electronegativity is 1.2. In a free form, berkelium is a silvery-white metal. Stable at a temperature below ∼1250 K is α-Bk with double hexagonal close-packed structure (hexagonal layers alternate 4 ), basic ABAC. . . ; space group P 63 /mmc (D6h parameters a = 0.3416 nm, c = 1.1069 nm at room temperature). Stable above ∼1250 K up to T melting ≈ 1290 K is β-Bk with hexagonal closepacked structure (space group F m3m, Oh5 ; parameter a = 0.4997 nm at room temperature after hardening). Density is 14.80 g/cm3 ; T boiling is about 2880 K. At low temperatures, α-Bk becomes antiferromagnetic with Néel point T N ≈ 22 to 34 K). In β-Bk, no magnetic ordering has been detected. Berkelium isotopes are used for research in nuclear physics and radiochemistry. Berkelium is highly toxic. BERNAL’S FLUID MODEL See Random close-packing model. BERYLLIUM, Be

A chemical element of Group II of the periodic system with atomic number 4 and atomic mass 9.01218. Natural beryllium consists of the stable isotope 9 Be with electronic conﬁguration 1s 2 2s 2 . The ionization energies are 9.323 or 18.21 eV. Atomic radius is 0.113 nm, Be2+ ion radius is 0.035 nm. It is chemically active; oxidation state is +2. Electronegativity is 1.47. In a free form, beryllium is a light bright gray metal, which is brittle under normal conditions. The properties of beryllium depend on its purity, grain size, texture and degree of anisotropy that depend on its pretreatment. Some properties change with an increase of pressure and temperature, and upon strong neutron irradiation (>1023 neutrons/m2 ). Beryllium crystallizes in two allotropic modiﬁcations. Below 1527 K, α-Be is stable (hexa-

110

BERYLLIUM ALLOYS

gonal close-packed lattice with parameters a = 0.2283 nm, c = 0.3584 nm at 300 K and impurity content no more than 1%; space group P 63 /mmc, 4 ). Above 1527 K up to T D6h melting = 1560 K, β-Be is stable (body-centered cubic with parameter a = 0.2546 nm at 1527 K; space group I m3m, Oh9 ). Bond energy of pure beryllium is 3.33 eV/atom at 0 K; density is 1.848 g/cm3 (at 293 K); melting heat is 11.7 kJ/mole; sublimation heat is 314 kJ/mole; T boiling = 2743 K; evaporation heat is 309 kJ/mole; speciﬁc heat is 1.80 kJ·kg−1 ·K−1 ; Debye temperature is 1160 K. Coefﬁcient of linear thermal expansion is 9.2·10−6 K−1 along the principal axis 6 and 12.4·10−6 K−1 perpendicular to it (at 300 K). Heat conductivity reduces from 230 W·m−1 ·K−1 to 178 W·m−1 ·K−1 in the temperature range 273 to 323 K; adiabatic coefﬁcients of elastic rigidity of α-Be monocrystal: c11 = 288.8, c12 = 20.1, c13 = 4.7, c33 = 354.2, c44 = 154.9 GPa at 298 K (within the range 423 to 1530 K c13 0 GPa). Bulk modulus is ≈109 GPa, Young’s modulus is ≈304 GPa, rigidity is ≈143 GPa; Poisson ratio is ≈0.056 (at 298 K); ultimate tensile strength is 0.196 to 0.539 GPa; relative elongation is 0.2 to 2%. Pressure treatment considerably improves mechanical properties; ultimate strength in stretching direction reaches 0.392 to 0.784 GPa; yield limit is 0.245 to 0.588 GPa; and relative elongation up to 4 to 12%; mechanical properties perpendicular to stretching undergo minimal change. Brinell microhardness is 1.18 GPa; impact strength is 0.001 to 0.005 GPa; transition temperature of commercially pure beryllium from brittle to plastic state is 473 to 673 K. Highly pure beryllium (above 99.9%) with grain size 90◦ (see also Uniaxial crystals). BICRITICAL POINT

A point on the phase diagram of a crystal where two curves of second-order phase transitions and one curve of a rst-order phase transition meet. The latter curve usually separates the regions of existence of two different ordered phases (see Multicritical point). BIEXCITON, exciton molecule A bound state of two excitons in semiconductors and insulators.

A biexciton in a semiconductor is a stable fourparticle complex containing two electrons and two holes. Since the effective masses of an electron me and a hole mh in semiconductors are close to each other, the biexciton stability problem has no small parameter for carrying out a power series expansion. Therefore, the adiabatic approximation widely used in molecular spectroscopy is inapplicable in this case; and the calculations are usually carried out with the help of the variational method. In the limit me /mh = 1, the biexciton stability problem is analogous to the positronium molecule problem. The binding energy of the positronium molecule is extremely small: M ≈ 0.02Ex where Ex is the binding energy of the positronium atom (electron–positron bound state analogous to hydrogen atom). For example, the biexciton binding energy in Ge and Si is ΔM 1 meV. Variational calculations of this

BIOLOGICAL CRYSTALS

binding energy in semiconductors with different energy band structures demonstrate that biexcitons are stable for arbitrary values of the ratio me /mh . In the limit me /mh → 0, corresponding to a hydrogen molecule, ΔM = 0.35Ex . Since the energy gain due to biexciton formation from two excitons is insigniﬁcant, from the thermodynamic viewpoint biexciton formation is likely only at low enough temperatures. The probability of formation is in proportion to the square of the exciton concentration; and the estimates show that this concentration should be very large. The most direct method for the detection and investigation of biexcitons is the analysis of their recombination emission spectra. The most probable process of radiative biexciton decay is via a single electron–hole pair recombination accompanied by the creation of a photon and a recoil exciton. The radiative decay of biexcitons was detected in the indirect-gap semiconductors Ge and Si. In direct-gap semiconductors, the recombination times are extremely short (10−9 s or less). Hence, the processes of binding excitons into biexcitons and the nonradiative decay of the latter takes place under highly nonequilibrium conditions with respect to both the phonon system and between the electron–hole components of the system itself. Therefore, to study the biexciton properties in direct-gap crystals experimentally, nonlinear optical methods were developed that are most efﬁcient under highly nonequilibrium conditions. The methods include the two-phonon resonance excitation of biexcitons, the induced one-phonon transformation of an exciton into a biexciton, as well as the two-phonon resonance Raman scattering of light (or hyper-Raman scattering) with participation of biexciton states. The efﬁciency of these processes in direct-gap semiconductors is associated with a very large value of the nonlinear susceptibility at two-phonon resonance in the biexciton state. This is the basis for nonlinear effects of the multiwave mixing (see Frequency mixing) and bistability with participation of biexcitons. With the help of these methods, biexcitons were detected and studied in a number of direct-gap semiconductors (CuCl, CuBr, CdS, etc.).

113

BIMETALS, bimetallic materials

Materials consisting of two different, tightly bonded metals or alloys. A distinctive feature of bimetals is a combination of various properties such as strength and thermal-environment resistance, wear resistance, or low electric resistance. Joining of bi- or multilayer metals occurs via the action of interatomic forces which bring the pure metal surfaces to a separation close to an interatomic one. The bimetals are obtained either using plastic deformation (rolling, pressing, pressure welding, drawing, diffusion welding) or without it (casting, electroslag welding, metallization by spraying, and so on). In industry, bimetals are used for preserving expensive metals or alloys, as well as materials with special properties. Bimetals containing metals (alloys) with different thermal expansion coefﬁcients are called thermobimetals. BINARY ALLOYS, double alloys Alloys formed from two component systems. Binary alloys are used when studying phase diagrams of the phase equilibrium and the phys-

ical, chemical, thermodynamic and other properties of alloys composed of two components. For example, binary alloys of the iron–carbon system, binary alloys based on nickel, and so on. These alloys include single-phase alloys and two-phase alloys, intermetallic compounds, interstitial alloys, and substitutional alloys, as well as various metallic materials regardless of the mode of their manufacture. A common feature is their two-component composition. For two-component alloys (differing in concentration) the term binary alloy system is used (e.g., the melt diagram of the binary system Al–Si). Alloys containing three or four components are called tri-component alloys and tetracomponent alloys, respectively. Alloys composed of four and more components are called multicomponent alloys. BIOLOGICAL CRYSTALS Crystals built of biological molecules (pro-

teins, nucleic acids or virus particles). Due to the enormous dimensions of biological macromolecules containing 103 –104 atoms, biological crystals have very large crystal lattice periods (5–20 nm) compared to ordinary crystals,

114

BIPHONON

Packing of molecules in a protein crystal.

the lattice periods in a virus reaching 100 nm or more. An important feature of biological crystals is that they contain, in addition to the macromolecules themselves, some of the host solution (35–80%), from which the molecules were crystallized, typically water with various ions (see Fig.). Many biological crystals exist solely in equilibrium with such solutions. Desiccation brings about the denaturation (structural decay) of molecules and the crystal as a whole. Regularity of the arrangement of molecules in biological crystals is determined by the electrostatic interaction of the charged atomic groups at the surface of the molecules, with van der Waals forces and hydrogen bonding playing a major role. The solvent molecules adjacent to the surface are arranged in order; those in the intermolecular space are disordered. The methods of crystallization of biological crystals are based on the variation of the temperature and oversaturation. To change the solubility, some particular salts, or organic solutes, etc., are introduced into the solution. The enormous dimensions of biological crystals allow one to directly observe their packing in the crystal lattice with the help of electron microscopy. X-ray diffraction also provides data on the most complicated spatial conﬁguration of the molecules composing the crystals, but the enormous number of reﬂections obtained (100,000) render the process of decoding them extremely complex. In addition to the true three-dimensional periodic biological crystals, there exist biological crystals with different types of ordering. Thus, deoxyribonucleic acid (DNA) forms textured gels, i.e. liquid crystals. Their X-ray structural analysis

allowed a spatial model of DNA to be constructed, and the nature of the genetic information transfer to be established. Some globular proteins (catalase and others) crystallize with the formation of tubes with monomeric walls built of molecules arranged according to spiral symmetry. Research of crystals of spherical viruses with the help of electron microscopy and X-ray analysis allowed one to establish the character of the mutual packing, and the structure of the protein molecules composing the virus shell. The latter are arranged in a virus particle according to icosahedral symmetry, with an axis of 5th order (see Crystal symmetry). BIPHONON A quasi-particle representing a bound state of two phonons, arising due to the anharmonic vibrations.

Both phonons move in the crystal as an integral whole, and are characterized by the same value of the wave vector. A biphonon inﬂuences phonon optical spectra of absorption and spectra of Raman scattering of light as a sharp maximum situated at an energy below the lower edge of the corresponding two-phonon band. The latter characterizes the crystal excitation region for the simultaneous creation of two phonons (the socalled sum process), or at the creation of a phonon of higher energy with simultaneous destruction of another one of lower energy (the so-called difference process). The separation of a biphonon peak from the two-phonon band and its intensity are determined by constants characterizing the anharmonicity, and by the density distribution of twophonon states. Biphonons are frequently observable in phonon spectra at low temperatures. BIPOLAR DIFFUSION The same as Ambipolar diffusion. BIPOLARON

A system consisting of two conduction electrons bound by a strong interaction with the medium; in other words, two bound polarons. The appearance of bipolarons is possible in crystals, amorphous materials, and liquids. If the macroscopic polarization dominates the interaction with the medium then the large dielectric constant of the medium favors the creation of bipolarons. The electron motion in a bipolaron is correlated; an essential feature is their space separation

BIPOLAR TRANSISTOR

inside the polarization potential well. The possibility of forming bipolarons was ﬁrst established analytically in ionic crystals and then extended to amorphous insulators, metals and other materials. In bipolarons the electrons with opposite spins are bound, which leads to the absence of paramagnetism of the free charge carriers. The experimental evidence of the existence of bipolarons was obtained in a series of oxide crystals with variable valence (e.g., Ti4 O7 ), and in some compounds of linear organic molecules. The space–time properties and energy scale of a bipolaron are essentially different from those in a Cooper pair. See also Bipolaron mechanism of superconductivity. BIPOLARON MECHANISM OF SUPERCONDUCTIVITY

A possible mechanism to explain supercurrent ﬂow through a crystal without resistance at low temperatures due to the super uidity of a charged Bose gas or a Bose u id of bipolarons. The elementary excitation spectrum in such a system of charged bosons possesses, due to the long-range Coulomb repulsion, a ﬁnite energy gap E0 = ωp at zero momentum (where ωp is the frequency of the collective plasma oscillations in the bipolaron gas). This also satisﬁes the Landau super uidity criterion, which in this case corresponds to superconductivity. The bipolaron mechanism of superconductivity differs from the Cooper pairing of the Bardeen–Cooper–Schrieffer theory (BCS) in that bipolarons of small and intermediate radii are separated in space, and are not expected to decay above the transition from the superconducting to the normal state. To estimate the critical temperature of such a transition, one can use the expression for the Bose–Einstein condensation tem2/3 perature T0 = 3.312 n0 /m∗B (where n0 is the

115

concentration and m∗B is the effective mass of the bipolarons) of an almost ideal charged Bose gas 1/3 ∗ >1 of high density under the condition n0 aB ∗ = ε 2 /(4e2 m∗ ) is the effective Bohr (where aB 0 B radius of a bipolaron with charge of 2e, and ε0 is the static dielectric constant of the crystal). An estimate T0 2–50 K was obtained for bipolarons of intermediate radius in ionic crystals with ε0 1 of SrTiO3 type at m∗B 10m0 (m0 is free electron mass) and n0 ≈ 1017 –1020 cm−3 , while T0 8–80 K for bipolarons of small radius with m∗B ≈ (100–1000)m0 at n0 1022 cm−3 . The bipolaron mechanism of superconductivity has been proposed theoretically for heavy fermions (CeCu2 Si2 , UBe13 , UPt3 ), semiconducting perovskites BaPb1−x Bix O3 and possibly the new high-temperature superconductor cuprates. BIPOLAR TRANSISTOR A semiconductor device with its active zone containing two semiconductor junctions separated

by a thin region called a base. The outer zones having the same conduction type are called the emitter and collector (see Fig.). In an n–p–n type transistor the minority current carriers of the base (electrons) diffuse through the p-type base region and penetrate the n-type collector region; in a p–n–p type bipolar transistor the minority current carriers (holes) diffuse through the n-type base region. A bipolar transistor is designed in such a way that small variations of the electric current or voltage could cause signiﬁcant current variations between the emitter and the collector. As to their design, bipolar transistors can be either homostructural, heterostructural, or have graded bands. Bipolar transistors serve for the generation and ampliﬁcation of electromagnetic oscillations, and for the control of voltage and current.

Structure (left) and energy diagram (right) of an n–p–n bipolar transistor showing the emitter (e), base (b) and collector (c) regions. The donor and acceptor energy levels are indicated by dashed horizontal lines.

116

BIRADICAL

BIRADICAL

A molecule containing two spatially separated radical centers (unpaired electrons), with the singlet–triplet energy splitting of the orbital state lower than or close to k B T . The appearance of biradicals in a solid causes changes in an electron paramagnetic resonance spectrum due to exchange interactions and dipole–dipole interactions. In chemical reactions, a biradical behaves as two independent, but joined together, free radicals. BIREFRINGENCE Refraction of light in anisotropic media (e.g., crystals), which results in its splitting into two

beams with different polarizations. It was discovered by E. Bartholin (1669) in calcite crystals. Birefringence is caused by the tensorial dependence of the polarization vector of the anisotropic medium on the light wave electric ﬁeld intensity. The result is that the polarization of light in the medium and the phase velocities of the waves (refractive indices) both depend on the direction of propagation. In optically inactive crystals, upon birefringence the two waves are locally polarized in mutually perpendicular planes (in the general case of an optically active crystal the waves are elliptically polarized) and they have different phase velocities. In single-optical-axis crystals one of the waves (ordinary ray) is polarized perpendicular to the main cross-section, i.e. the planes which pass through the direction of the light wave and the optical axis of a crystal, and the other wave (extraordinary ray) is polarized parallel to it. Refraction of the ordinary wave is similar to refraction (see Refraction of light) in an isotropic medium since the ray vector coincides with the wave vector and the refraction index does not depend on the direction of propagation. For the extraordinary wave the common law of refraction is not satisﬁed: the wave and ray vectors do not coincide, and the refraction index n0 depends on the direction of propagation. For light propagation along the optical axis there is no birefringence. Biaxial crystals are characterized by three refraction indices, and they have two directions (two optical axes), along which there is no birefringence. The phase velocities of both waves depend on the direction of propagation, and both waves, upon refraction, may emerge from the plane of incidence.

Birefringence is possible not only in naturally anisotropic media, but also in media with an induced anisotropy caused by external ﬁelds: electrical (Pockels effect, Kerr effect), magnetic (Voigt effect), and acoustical. Phenomena similar to birefringence have also been observed outside the optical range of the electromagnetic spectrum. See also Self-induced light polarization change. BISMUTH (Lat. Bismuthum), Bi

Chemical element of Group V of the periodic table; atomic number 83, atomic mass 208.98. Natural bismuth consists of one stable isotope 209 Bi. Electronic conﬁguration of outer shells is 6s 2 6p3 . Ionization energies are 7.289, 16.74, 25.57, 45.3, 56.0 eV. Atomic radius is 0.182 nm, radius of Bi3+ ion is 0.120 nm, of Bi3− ion is 0.213 nm. Electronegativity is ≈1.95. In the free form Bi is a silvery metal with a pink tint. Crystalline lattice is rhombohedral with the following parameters: a = 0.47457 nm and α = 57◦ 14 13 . Its density is 9.80 g/cm3 (at 293 K); density of the liquid form is 10.27 g/cm3 (at 544.4 K); T melting = 544.4 K, T boiling = 1833 K. Speciﬁc heat is 0.129 (at 293 K), in liquid state 0.142 (at 544.4 K), 0.148 (at 673 K), 0.166 kJ·kg−1 ·K−1 (at 1073 K); thermal coefﬁcient of linear expansion is 13.3·10−6 K−1 , volume expansion of metal upon solidifying +3.32% (at 544.4 K); thermal conductivity coefﬁcient is 8.374 W·m−1 ·K−1 (at 293 K), 15.491 (at 673 K); heat of melting is 11.38 kJ/mole; heat of evaporation 179 kJ/mole. Speciﬁc electrical resistance is 1068 μ·m (at 293 K), 1.602 (at 373 K), 1.289 (at 573 K), 1.535 (at 1053 K). The transition temperature T c of a superconducting thin ﬁlm state is ≈7 K. Under the inﬂuence of a magnetic ﬁeld the electrical resistance of Bi increases more than that of other metals so it is used for the measurement of strong magnetic ﬁelds. The tensile strength is 4.9 to 19.6 MPa, elastic modulus is 31.37 GPa, rigidity 12.35 GPa, Brinell hardness is 94.2 MPa, Mohs hardness is 2.5. Adiabatic elastic moduli of Bi in the hexagonal system, 3m (D3d ) class (room temperature): c11 = 63.7, c12 = 24.88, c13 = 24.7, c14 = 7.17, c33 = 38.2, c44 = 11.23 GPa. In the temperature range 423 to 523 K, bismuth compresses in a comparably easy manner. Bismuth is a diamagnetic metal with magnetic susceptibility −1.35·10−9 (upon melting the susceptibility

BLISTERING

decreases 12.5 times). Cross-section for thermal neutron capture is not high in Bi (0.034 barn). Bismuth is used for the production of low-melting alloys (e.g., Wood’s metal alloy with melting point of 343 K). Bismuth alloys are used in the helices of devices for measuring strong magnetic ﬁelds, and it also serves as a heat-transfer agent in nuclear reactors. BISTABILITY

A property whereby a system has two stable states in a certain region of variation of its parameters. The existence of bistability is connected with nonlinear properties of the system, and produces hysteresis during a fast enough variation of the parameters. It is exempliﬁed by optical bistability, polarization optical bistability, an N- or S-shaped current–voltage characteristic, the magnetic polarization of a ferromagnet, in a magnetic ﬁeld, etc. Nonlinear systems may exhibit more than two stable states (multistability). BITTER PATTERN See Magnetic powder pattern. BLACK-AND-WHITE GROUPS The same as Shubnikov groups. BLAHA–LANGENECKER EFFECT (F. Blaha, B.-Z. Langenecker, 1935)

Reduction of the force needed for plastic deformation of a specimen under simultaneous action of static and alternating loads.

117

The effect is observed in technological processes involving the shape-changing of metals (such as drawing, punching, rolling, and so on). The effect is especially noticeable when using ultrasound (see Ultrasonic treatment); in this case, the reduction of static stress depends on the ultrasound intensity, the nature and the condition of the material, the temperature, and other conditions. The effect of the ultrasound is explained by a local absorption of the energy of the high-frequency oscillation by various defects of the crystalline structure (see Defects in crystals), which facilitates the multiplication of dislocations and vacancies, as well as their motion in the crystal. BLISTERING

An appearance of blisters on a crystal surface under bombardment with atoms (ions) of inert gases, protons, and other particles. The blisters “ripen” with an increase in dosage (see Dosimetry) up to a stage when the blister dome breaks due to the increased pressure inside it. A new generation of blisters can develop on the uncovered area. The subsequent stages of the blistering are shown in the ﬁgure. The phenomenon of blistering is caused by migration of irradiationinduced vacancies and vacancy pores towards the surface. The mechanical stresses arising at embedding of the bombarding ions into the subsurface layer can also induce blistering. If the defect density is sufﬁciently uniform along the surface, the scabbing of thin plates off the surface of the irradiated material takes place instead of blister formation. The blistering and ﬂaking phenomena lead

Blistering process.

118

BLOCH EQUATIONS

to strong surface erosion of irradiated material at high irradiation doses. BLOCH EQUATIONS (F. Bloch, 1946)

Phenomenological equations describing the magnetic properties of ensembles of electrons (γ < 0) and nonzero-spin nuclei (γ > 0) in external magnetic ﬁelds:

χ = (ω0 − ω)T2 χ ,

Mx i + My j dM = γ (M × B) − dt T2 Mz − M0 − k, T1

χ = (1)

where Mx , My , Mz are the components of magnetization vector M; M0 is the equilibrium value of Mz ; i, j and k are the unit vectors of the laboratory coordinate system; B = kB0 + i2B1 cos ωt , B0 is the constant magnetic ﬁeld component directed along z axis; ω is the frequency; and B1 is the amplitude of alternating magnetic ﬁeld (B0 B1 ); γ is the gyromagnetic ratio. The constant T1 is called the longitudinal or spin–lattice relaxation time and T2 is the dephasing time, also referred to as the transverse or spin–spin relaxation time. In the general case, T1 is unequal to T2 (T1 T2 ) since T1 characterizes the rate of establishing thermal equilibrium between the spins and the lattice, while T2 is related to rate of establishing thermal equilibrium within the spin system, and this latter is equivalent to the decay rate of the phase coherences between precessing spins (as a result of the interaction between each other and with their environment, the spins precess in different local ﬁelds). The Bloch equations are based on the following reasoning. In an arbitrary uniform magnetic ﬁeld B the equation of motion of the magnetization vector M of the ensemble of free spins has the form dM/dt = γ (M × B). It is postulated that: (i) in a constant magnetic ﬁeld Bz , the longitudinal magnetization Mz relaxes to M0 in an exponential manner, i.e. satisﬁes the equation dMz /dt = −(Mz − M0 )/T1 ; (ii) transverse components Mx and My decay exponentially to zero as dMx Mx , =− dt T2

dMy My ; =− dt T2

(iii) in an external magnetic ﬁeld (comprised of a strong constant and weak alternating components) the relaxation motion of the magnetization vector is superimposed on the motion of free spins. Under the conditions of resonance, the stationary solutions of Eqs. (1) lead to the following expressions for the real (χ ) and imaginary (χ ) parts of the magnetic susceptibility:

(2)

−1 1 , γ M0 T2 1 + (ω − ω0 )2 T22 + S 2

where ω0 = γ B0 , χ determines the Lorentzian shape of the line with a half-width at a half-height of Δ = (1 + S)1/2 /T2 ; and the saturation factor (see Saturation effects) S = γ 2 B12 T1 T2 indicates the dependence of the line shape on the alternating ﬁeld intensity. In the absence of saturation (S 1), the half-width is determined by the spin– spin relaxation time T2 . The Bloch equations are also used for the analysis of pulsed experiments. One can obtain Eqs. (1) from the general theory of relaxation (see Bloch–Red eld theory). For twolevel systems they are valid if alternating ﬁelds are small and there are no spin–spin interactions. In solids the value of T2 is often estimated from the width. In this case Eqs. (1) lead to a discrepancy with the experimental data in the limit of strong saturation. Despite the limits to their applicability, the Bloch equations play an important role in elucidating many aspects of nuclear magnetic resonance and electron paramagnetic resonance in solids. BLOCH FUNCTION See Bloch theorem. BLOCH–GRÜNEISEN FORMULA (F. Bloch, E. Grüneisen, 1930)

An interpolating expression describing the temperature dependence of that part of electric resistance of metals ρT that is caused by electron scattering by lattice vibrations (phonons): 5 Θ/T z5 dz T ρT = 4 ρ0 , z Θ (e − 1)(1 − e−z ) 0

(1)

BLOCH LINE

where Θ is the Debye temperature, and ρ0 is a constant independent of temperature. In the simplest case of a spherical Fermi surface, the value of ρ0 is ρ0 =

ε2 3π m2 , 2 2 e n M0 v0 kΘ

(2)

where m is the electron effective mass, M0 is the atomic mass of a metal atom, v0 is the volume per atom, n is the density of conduction electrons, ε is a particular energy parameter (in the simplest case, the strain potential) characterizing the electron–phonon interaction; ε ∼ 1–10 eV. At high temperatures (T Θ), Eq. (1) has the form ρT = (T /Θ)ρ0 , i.e. it describes an ordinary linear growth of the metallic resistance with increasing temperature. At low temperatures (T Θ), Eq. (1) yields the wellknown Bloch law ρT ∼ T 5 , where ρT = 497.6(T /Θ)5 ρ0 . For a majority of simple metals the parameter Θ evaluated from Eq. (1) is in good agreement with the Debye temperature obtained from measurements of the speciﬁc heat. BLOCH LAW, three halves power law (F. Bloch, 1930)

The temperature T dependence of spontaneous magnetization Ms of ferromagnets in the temperature range signiﬁcantly lower than Curie point Θ, but higher than the magnon activation energy:

119

BLOCH LINE

A linear inhomogeneity of a 180◦ magnetic domain wall (Bloch wall) that separates wall re-

gions with different directions of magnetization rotation (see Fig.). The z axis is the Bloch line. A Bloch line cannot end anywhere in the domain wall, it either forms a closed ring, or terminates at the surface of the magnetic substance, i.e. the medium. The domain wall thickness decreases near the Bloch line, as shown. Bloch lines are distinguished according to their orientation. Vertical Bloch lines are directed normally to the surface of the magnetized material, and exist in domain walls of materials with magnetic bubble domains. They can be detected with the help of direct methods, such as electron microscopy or, in some cases by magneto-optic methods (see Magnetic domain characterization), and by the deformation of a moving domain wall at the location of an accumulation of vertical Bloch lines. Magnetic bubble domains with a large number of vertical Bloch lines (see Rigid magnetic bubble domain, Dumbbell domain) possess anomalous dynamic properties. S. Konishi (1983) proposed to use these lines for solid-state systems capable of superdense magnetic information recording. Horizontal Bloch lines that are directed parallel to the sample surface, as well as Bloch lines of a more involved shape, can arise during the motion of a twisted domain wall (see Domain wall twisting). Horizontal Bloch lines

T 3/2 , Ms = Ms0 1 − α Θ

where M s0 is the maximum value of M s at T = 0 K, and α is a constant which is speciﬁc for a given substance. This formula represents the ﬁrst terms of the expansion of M s (T ) in powers of T /Θ. The subsequent terms of the series are negligible (at T < Θ) and, as experiments show, the Bloch law is satisﬁed well up to T ≈ Θ/2. The decrease of M s with increasing T is a result of the disturbance of the ordered orientation of atomic (spin) magnetic moments in ferromagnets due to the thermal excitation of magnons. Their number grows as T 3/2 with increasing temperature, in accordance with the equation.

Distribution of magnetization indicated by solid arrows outside and within a domain wall with vertical (along z) Bloch lines; light arrows indicate directions of magnetization rotation.

120

BLOCH POINT

play an important role in the formation of the phenomenon of ballistic aftereffect in the motion of magnetic bubble domains. BLOCH POINT

A point inhomogeneity, a singular point of the magnetization M(r) at the merging of two Bloch lines of different signs in a magnetic domain wall.

The magnetization on a closed surface surrounding a Bloch point takes on all possible values. Thus, m = M/M s is equal to +ez and −ez far from the domain wall, to +ey and −ey in the middle of the domain wall far from the Bloch line, and to +ex and −ex in the middle of Bloch line segments of opposite sign (see Fig.). Hence, when approaching a Bloch point, the direction of magnetization m depends on the direction of approach, thus producing a “hedgehog”-type singularity of the magnetization ﬁeld (see Topological inhomogeneity). The following distribution corresponds to this singularity at a < r < Δ (a is the interatomic distance, Δ is the domain wall thickness): r (1) m=± , r where the different signs determine the sign (i.e. topological charge) of a Bloch point. There are other possible distributions that can be obtained

Distribution of magnetization indicated by arrows in a domain wall with a Bloch point BP crossed by Bloch lines BL-1 and BL-2.

from Eq. (1) by a uniform rotation. (The Bloch point in Fig. takes the form m = r/r after the rotation of m by π/2 about the y axis.) In materials with strong uniaxial magnetic anisotropy, the loss of domain wall energy due to the presence of a Bloch point is not signiﬁcant. Bloch points must always arise under certain distributions of the magnetization. Bloch points and their displacements under the action of an appropriately directed magnetic ﬁeld (along x axis) are detectable in domain walls of materials with magnetic bubble domains by the deviation of the direction of domain motion from the direction of the magnetic ﬁeld gradient (see Rigid magnetic bubble domain). BLOCH–REDFIELD THEORY

A magnetic resonance theory describing the time evolution of a spin system, located in an external magnetic ﬁeld, and interacting with its molecular environment (with the lattice). The main result of the theory is the Markovian kinetic equation for the spin density matrix. A consistent quantum-statistical derivation of the kinetic equation was ﬁrst presented by F. Bloch and R.K. Wangness, then Bloch generalized the theory for alternating magnetic ﬁelds of arbitrary magnitude. Later A.G. Redﬁeld put forth a semiclassical theory of relaxation where an approach to the calculation of the kinetic equation coefﬁcients was treated for the ﬁrst time. The basic physical concepts of the Bloch and Redﬁeld theories are the same. Later, both theories were described within the framework of a general formalism by other authors. Let a closed region comprise a spin system and a lattice with the Hamiltonian H = Hs + Hs (t) + Hsf +F where Hs is the time-independent Hamiltonian of the spin system, Hs (t) is the interaction operator of the spin system with alternating mag netic ﬁelds, Hsf = α uα vα is the spin–lattice interaction operator, uα are the lattice operators, vα are the spin operators, F is the Hamiltonian of the lattice. The exact equation of motion for the density matrix ρ of the closed system, idρ/dt = [H, ρ], is iterated in the interaction representation, and the inﬁnite series obtained is truncated at the second term (spin–lattice interaction considered as small perturbation). Then the spin density matrix evolves with the expression: σ = Trq ρ where the

BLOCH WALL

trace (Tr) of the matrix is taken over the lattice states. The kinetic equation for elements σmn has the following form: dσmn dt = i[σ, Hs + Hs (t)]mn + (2Γmkln σkl − Γklmk σln − Γlnkl σmk ). kl

(1)

Here the indices m, n, k, l enumerate the energy levels of Hamiltonian Hs ; jαβ (ωmk )vβmk vαln Δ(ωmk +ωln ), Γmkln = π

121

the density matrix σ changes insigniﬁcantly within the time tl , thus allowing one to apply perturbation theory); (iv) alternating magnetic ﬁelds are small; γ B1 τc−1 , γ B0 , where B1 is the amplitude of the external alternating magnetic ﬁeld, B0 is the amplitude of the externally applied magnetic ﬁeld, and γ is the gyromagnetic ratio; (v) the interaction between the lattice and the spin system results in a small shift of the levels of the latter that is ignored in Eq. (1); and (vi) the relaxation coefﬁcients Γ are time-independent and comparable to the reciprocals of the relaxation times.

αβ

where jαβ (ωmk ) is the Fourier transform of the lattice correlator: jαβ (ωmk )

=

−βFr δ(ω mk + ωrr ) r,r uαr r uβrr e , −βF 2πTrq e

where ωr r are the lattice eigenfrequencies; ωmk are the eigenfrequencies of the spin system; vβmk and vαln are the matrix elements with respect to eigenfunctions of Hamiltonian Hs ; uαr r and uβr r are the matrix elements of eigenfunctions of operator F ; β = /(k B T ), where T is the lattice temperature, Fr is the energy of rth lattice level. One must retain on the righthand side of Eq. (1) those Γmkln for which |ωmk + ωln | τc−1 . This is formally achieved by the introduction of the Heaviside step function Δ(x) = 1 at |x| < τc−1 and Δ(x) = 0 otherwise, where τ c is the lattice correlation time (perturbations in the lattice disappear within time τ c ). The derivation of the equation requires a number of assumptions: (i) the lattice stays close to thermal equilibrium; (ii) the inﬂuence of the spin system on the lattice is negligible, since the lattice has many more degrees of freedom than the spin system (ρ = σρf , where ρf is the equilibrium density matrix of the lattice); (iii) there exists a time interval t such that

t τ c and simultaneously t τ r , where τ r is the shortest relaxation time of the spin system (if the latter condition is met then

It follows from the relation Γmkln = Γlnmk exp(βωln ) ≈ Γlnmk exp(βωkm ) that in the absence of alternating magnetic ﬁelds, the solutions of Eq. (1) are elements of the equilibrium spin density matrix, i.e. due to the relaxation the spin system equilibrates with the lattice. Eq. (1) describes the magnetic resonance and the relaxation of magnetically dilute spin systems. BLOCH THEOREM

One of the most important theorems in solid state physics, which states that the intrinsic states of a particle in a periodic potential V (r) satisfying condition V (r + t) = V (r) (where t is the constant distance vector called the directlattice vector) can be characterized by two quantum numbers, viz., the band number λ and a realvalued vector k called the quasi-wave vector (lattice wave vector or crystal momentum). The wave function Ψkλ (r) called the Bloch function satisﬁes the condition Ψkλ (r + t) = Ψkλ (r) exp(ikt); and can be written as Ψkλ (r) = ukλ (r) exp(ikt) where ukλ has the symmetry of the potential, so that ukλ (r + t) = ukλ (r). The function Ψkλ (r) can also be written as a linear combination of Wannier functions Φλ (r), i.e. Ψkλ (r) =

ikr R e Φλ (r − R), where the set of points R transforms to itself upon displacement by the vector t , i.e. it possesses the symmetry of the potential. BLOCH WALL See Magnetic domain wall.

122

BLOCH WAVE FUNCTION

BLOCH WAVE FUNCTION See Bloch theorem. BLOCK STRUCTURE Partitioning a crystal into regions (blocks)

slightly disoriented relative to each another (disorientation angles are on the order of a few minutes of arc). Other terminologies are mosaic structure and blocks of mosaics (see Mosaic crystals). A block structure comprises disordered regions separated by closed small-angle boundaries in the form of dislocation interlacements, skeins, tangles, nets and dislocation walls of various structural and dislocation compositions. The regions contain both a cellular structure and a variety of dislocation structures such as individual dislocations, dislocation dipoles, multipoles, clusters, interlacements, wisps, nets, walls, and so on. The boundaries may be thin or thick, dense or rareﬁed, etc. The nets, boundaries, and walls may be regular or irregular; the networks may be hexagonal, tetragonal, etc. Incomplete (i.e. either forming or decaying) boundaries are a common occurrence. Depending on the dislocation composition and structure, the boundaries may be twisting or inclination ones, or a mixture of different varieties. The blocks may be equiaxial or nonequiaxial textured (see Texture). Block structures with smallangle boundaries composed of fairly regular nets and walls are often called polygonized structures. If the block size is commensurable with the grain size in a polycrystal, or with a single crystal size, the blocks are often called subgrains. The block size can vary from 0.1 to 10 μm. BLUE BRITTLENESS Lowering of the plasticity of unhardened construction steel at temperatures of blue color ir-

ridescence (300–500 ◦ C). It is responsible for the hardening of ferrite at temperatures about 300 ◦ C under conditions of static loading, and the formation of aggregations of impurity atoms which enhance its brittleness at temperatures about 400– 500 ◦ C under conditions of dynamic loading. In this case the plasticity is reduced owing to the formation of Cottrell atmospheres around dislocations because of the sharp growth of the diffusion rate as the temperature rises. In addition, under

conditions of shock loading, the velocity of dislocation motion exceeds that of impurity atom atmospheres. The latter start to lag behind the dislocations, forming elongated aggregations of impurity atoms, which extend in the direction of the steel plastic ﬂow. The presence of such aggregations in steel ferrite increases the alloy brittleness. Blue brittleness is reduced in steel by introducing elements linking interstitial atoms in carbides and nitrides. BLUE PHASES of liquid crystals Phases existing in a narrow temperature range

(1–0.1 ◦ C in order of magnitude) between a liquid phase and a cholesteric phase (see Cholesteric liquid crystal), possessing a spatial three-dimensional periodicity, and formed by bilaterally asymmetric elongated molecules. Three blue phases are known, designated as BPI, BPII, and BPIII, with no translational long-range order present in the highest-temperature phase BPIII of the group (see Long-range and short-range order). In view of the bilateral symmetry of phases BPI and BPII, a coil twisting is locally advantageous in two directions (in spite of the single direction where it takes place in a cholesteric). Therefore, a three-dimensional lattice of linear defects (disclinations) with a period 0.5 μm appears in the system. Thus, blue phases are the analogues of ordinary solid crystals where the structural elements are not the individual atoms or molecules, but the cells of the disclination network. There also exist some other models of blue phases. The positions of the molecules themselves are not ﬁxed; only their orientations are conserved at every point. Despite the lack of any direct proof of the existence of the disclination lattice in a blue phase, there are some indirect effects arguing in favor of the model, such as the increase of the lattice period with a decrease in the temperature. Due to a periodic structure, the BPI and BPII are able to form well-faceted monocrystals, and also to selectively scatter light in a visual spectral range, thus acquiring the blue color that gives them their name. Two optical characteristics of the BPI and BPII phases are the strong rotation of the light polarization plane (arising due to a coil structure) and the lack of linear double refraction (due to the cubic form of the disclination network cells). Although blue phases

BOGOLYUBOV METHOD

have been well known since the discovery of liquid crystals in 1888, nowadays these phases are among the least studied liquid crystals. BODY-CENTERED LATTICE, I -lattice

A lattice whose unit cell parallelepiped contains an extra site in the cell center (see Bravais lattices) as well as the sites at the vertices. In addition to the three basic translations a, b, c, the lattice possesses a further translation t = (a + b + c)/2. The latter can appear only in rectangular parallelepipeds; therefore, body-centered lattices exist only in orthorhombic, tetragonal, and cubic crystallographic systems. In triclinic and trigonal crystal systems the I-lattice reduces to a smaller primitive lattice (see Primitive parallelepiped). In a monoclinic crystal system, this is a base-centered lattice with the unit cell volume and other basis translations half as large. In the hexagonal lattice case, the appearance of the translation t leads to a lowering of the symmetry to that of a monoclinic base-centered lattice. Considering the point symmetry of the sites, the body-centered lattice belongs to the body-centered Bravais groups. BOGOLYUBOV CANONICAL TRANSFORMATIONS

See Canonical transformation method. BOGOLYUBOV–DE GENNES EQUATIONS (N.N. Bogolyubov, 1958; P.G. de Gennes, 1963)

Equations of the mean eld approximation in the theory of superconductivity that determine the energy eigenvalues ελ and the correspond (r) of Boing two-component wave functions uv λ(r) λ golyubov quasi-particles (see Bogolyubov method) in a spatially inhomogeneous state of a superconductor described by the order parameter Δ(r) = g(s −s ). Here s (r) is the annihilation operator of an electron with spin s, and g is the matrix element of the effective electron–electron interaction in Bardeen–Cooper–Schrieffer theory. These equations have the form: 0 uλ (r) + Δ(r)vλ (r) = ελ uλ (r), H ∗ vλ (r) + Δ∗ (r)uλ (r) = ελ vλ (r), −H 0

123

where 0 = 1 −i∇ − eA(r) 2 + U (r) − E F H 2m is the one-electron Hamiltonian of the normal state of a metal, m is the electron mass, A(r) is the magnetic ﬁeld vector-potential, U (r) is the effective one-particle potential for the electrons in the metal, and E F is the Fermi energy. In the thermodynamic equilibrium state, the value of Δ(r) satisﬁes the self-consistency condition ελ . uλ (r)vλ∗ (r) tanh Δ(r) = g 2kB T λ

The Bogolyubov–de Gennes equations were used to solve spatially nonuniform problems of superconductivity theory such as, e.g., calculation of the upper critical eld B c2 (T ), ﬁnding the excitation spectrum in the vortex lattices, determining the boundary conditions in proximity effect theory, elucidating particular features of the reﬂection of quasi-particles from a “normal metal– superconductor” interface (see Andreev re ection of quasi-particles), ﬁnding the excitation spectrum in S–N–S contacts, etc. BOGOLYUBOV METHOD in the theory of superconductivity (N.N. Bogolyubov, 1958)

A ﬁeld theory method for calculating the ground state energy and the spectrum of single particle and collective excitations in superconductors. The initial Hamiltonian of the electron and phonon subsystems of a metal was diagonalized using the unitary transformations of creation and annihilation operators of bosons and fermions (see Canonical transformation method) and the principle of renormalization, i.e. the compensation of divergent Feynman diagrams by a perturbation theory series. The Bogolyubov method is an alternative to the variational method in Bardeen– Cooper–Schrieffer theory and, unlike the latter, allows a consistent treatment of collective effects and the Coulomb interaction in superconductors. In particular, within the framework of the Fröhlich Hamiltonian for the electron–phonon interaction, this method was used to obtain in the

124

BOGOLYUBOV–TOLMACHYOV LOGARITHM

weak coupling limit, for the ﬁrst time, an equation for the energy gap parameter Δ in the spectrum of a superconductor taking into account effects of retardation. In addition, with the help of the Bogolyubov method, a further weakening of the screened electron–electron repulsion was shown to exist (see Bogolyubov–Tolmachyov logarithm), which facilitates Cooper pairing due to the electron–phonon interaction. When the Bogolyubov method was applied to collective excitations involving undamped branches in the energy range √ ω < 2Δ with a linear dispersion law ωq = qv F / 3 (where v F is the Fermi velocity), they were found to exist in neutral superﬂuid Fermi systems. That branch represents a Goldstone mode. In charged Fermi systems with longrange Coulomb repulsion (electrons in a metal), the branch transforms into plasma oscillations with the frequency ωq = 0 at q → 0. BOGOLYUBOV–TOLMACHYOV LOGARITHM (N.N. Bogolyubov, V.V. Tolmachyov, 1958) The logarithm of the ratio of the Fermi energy in metals E F ∼ 1–10 eV to the mean energy of phonons ωD ∼ 0.1–0.01 eV (ωD is the Debye frequency) that characterizes the extent of the ef-

fective weakening of the Coulomb repulsion between the electrons in a superconductor: c = V

Vc , 1 + N(0)Vc ln[EF /(ωD )]

where V c is the matrix element of the screened Coulomb interaction that is averaged over the Fermi surface, and N(0) is the density of states at the Fermi level. The extra (relative to screening) weakening of the repulsion is caused by the decreased probability of the appearance of two electrons within the limits of the screening region due to Coulomb scattering. It facilitates electron Cooper pair formation via an effective attraction, which results from virtual phonon exchange. BOHR MAGNETON See Magneton. BOHR RADIUS

The radius a B of the orbit of an electron in the ground state of a hydrogen atom.

More generally, the distance between the center of the hydrogen atom and the maximum of the quantum-mechanical probability for detecting an electron; or the distance through which the electron wave function reduces by the numerical factor of e = 2.71828. The Bohr radius has the value a B = 4πε0 2 /(me2 ) = 5.2918·10−11 m, where m and e are the electron mass and charge, respectively, = h/(2π) is the reduced Planck constant. In the physics of insulators and semiconduc∗ is used which tors the effective Bohr radius aB differs from the Bohr radius a B with m replaced with the effective mass of an electron in a crystal √ and e replaced by the effective charge e∗ = e/ ε, where ε is the relative dielectric constant. The effective Bohr radius determines the approximate ∗ n2 ) dimensions and energy, En = −e∗2 /(8πε0 aB (where n is the principal quantum number), of shallow hydrogen-like centers and Wannier–Mott excitons in semiconductors. It is a convenient scale for expressing the dimensions of localized electron states in nonmetallic crystals. BOHR–VAN LEEUWEN THEOREM (N. Bohr, 1911; generalized by J. van Leeuwen, 1919)

A theorem of classical statistical physics, which states that the magnetization of a system of charged particles in a constant external magnetic ﬁeld under the conditions of statistical equilibrium is equal to zero. The theorem demonstrates that it is impossible, within the framework of the classical statistical mechanics of charged particles, to explain ferromagnetism, paramagnetism and diamagnetism. As was shown later, the magnetism of a substance is caused by quantum properties of the particles comprising it. BOLOMETER

A device for measuring the radiated energy (power) in the infrared and optical wavelength ranges. It is in common use for various detection schemes with narrow ranges of extreme sensitivity to particular excitations. It was ﬁrst used by S. Langley (1880) for measurements in the IR range of the solar spectrum. The principle of bolometer operation is based on the change of the resistance of the thermosensitive element under the action of radiation. Bolometers are nonselective optical radiation detectors. To

BOLTZMANN EQUATION

obtain equivalent spectral sensitivity in a given range, absorbing coatings are applied to the sensitive elements of the bolometer. There are metallic, semiconductor (thermistor) and insulator bolometers. The use of cryogenic effects allowed producing cooled bolometers based on the conduction of shallow levels in semiconductors, as well as superconducting (isothermal and nonisothermal) bolometers. BOLTZMANN CONSTANT (L. Boltzmann)

One of the fundamental physical constants, a parameter of the statistical Boltzmann distribution and Gibbs distribution. Through them, the Boltzmann constant k B enters various thermodynamic relations, for example, it relates the thermodynamic probability W of a system state to the entropy S through the expression S = k B ln W , and determines the mean thermal energy k B T /2 of a particle per degree of freedom. The gas constant R involved in the equation of state for one mole of the ideal gas, pV = RT (p is pressure, V is gas volume), is related to the Boltzmann constant by k B = R/N A , where N A is the Avogadro number. The standard value based on the 1986 CODATA recommendations is k B = 1.38066·10−23 J/K. BOLTZMANN DISTRIBUTION A distribution function of coordinates and momenta for particles or quasi-particles of an ideal

nondegenerate gas in the state of thermodynamic equilibrium. The probability dW of a particle to have a momentum in a range p ⇒ p + dp and a coordinate in a range r ⇒ r + dr is related to the Boltzmann distribution fn (r, p) by dW (r, p) = fn (r, p) dr dp, where in the classical case we have the approximation ε(p) + U (r) . (1) fn (r, p) = A exp − kB T Here ε(p) is the kinetic energy, U (r) is the potential energy, k B is the Boltzmann constant, and A is the normalization factor found from the condition that the probability of a particle to be present in the phase space equals unity, i.e. W = dW = 1. Sometimes the following expression obtained by

125

integrating Eq. (1) over all momenta p is referred to as the Boltzmann distribution function: U (r) f (r) = A exp − , kB T while Eq. (1) is called the Maxwell–Boltzmann distribution. Integration of Eq. (1) over coordinates yields the Maxwell distribution of velocities. In a quantum description of particles characterized by a set of single-particle energy levels Ei , the Boltzmann distribution takes the form μ − Ei , (2) ni = exp kB T where ni is the average number of particles in the state with energy Ei , μ is the chemical potential of the system that acts as the normalization factor

determined by setting the sum i ni equal to the total number of particles, N . The Boltzmann distribution is the high temperature limiting case of the more accurate Bose–Einstein and Fermi–Dirac distribution functions (see Bose–Einstein statistics, Fermi–Dirac statistics) that take into account the quantum character of particle motion, and this limiting case is valid for an ideal gas with a small density of particles at high temperatures. In the physics of semiconductors, the Boltzmann distribution is widely used in the statistics of a gas of quasi-particles (electrons and holes) to determine their equilibrium concentrations and other speciﬁc parameters. BOLTZMANN EQUATION (L. Boltzmann, 1872) An integro-differential kinetic equation that

provides the time (t) evolution of the one-particle distribution function (f ) of a low-density monatomic gas. The Boltzmann equation has the form ∂f 1 + (p, ∇x f ) + (F, ∇p f ) = ρLp (f, f ), ∂t m where f (x, p, t) is the probability density function in the phase space of coordinates and momenta of a particle (x, p), m is the particle mass, F is the external force ﬁeld applied at the point (x, p) of the phase space, and ρ is a dimensionless parameter proportional to the mean density of gas particles. The collision operator (or collision

126

BOND

integral) Lp has the following form: 1 Lp (f, f ) = dp dσ |p − p | m × f (p∗ )f (p ∗ ) − f (p)f (p ) , where the explicit dependence of the function f on the coordinates and time is omitted, and dσ is the differential cross-section which includes conservation laws of both energy and momentum. Momenta p∗ , p ∗ can be found from solving the scattering problem for two particles with incident momenta p and p and a certain impact parameter, colliding in accordance with the laws of classical mechanics. When deriving the Boltzmann equation, the evolution of the function f (x, p, t) within a small time interval is assumed to be determined by its value at a given instant of time t by means of the free motion of gas molecules and their pairwise collisions, provided the interaction time during the collision of two gas particles is much smaller than their mean free path time. The operator Lp is constructed taking into account the number of particles in a phase volume element. The Boltzmann equation is derived from the Liouville equation in the lowest-order approximation using an expansion in powers of the density. If a system is in statistical equilibrium the collision integral vanishes, and the Maxwell distribution will be a solution to the Boltzmann equation. BOND

See Chemical bonds, Covalent bond, Hydrogen bond, Ionic bond, Ionic-covalent bond, Metallic bond. BOOJUM A point defect in the ﬁeld of a director at the boundary of a nematic (see Nematic liquid crystal).

Boojum-induced elastic distortion spreads over the entire bulk medium. Displacement of a boojum into the bulk is energetically unfavorable because a boojum in this case would be a point defect connected to the surface, i.e. a disclination. The director distribution in the vicinity of a boojum depends on the orientation of nematic molecules near the boundary. When this orientation changes, e.g., as shown in the ﬁgure, from a tangential orientation to a normal one, a boojum can either disappear or transform into a hedgehog and move from the sur-

Change in the director distribution during the transformation of a boojum into a hedgehog (above), and into a uniform state (below), during the variation of the director angle relative to the surface. Each distribution is axially symmetric, and the ﬁgure presents sections in a vertical plane.

face to the interior. Experimentally, boojums are observable in plane textures of liquid crystals in the form of defect points at the sample surface as well as in spherical nematic drops. The boojum was ﬁrst studied by N.D. Mermin (1976) in superﬂuid 3 He-A. The nature of the ordering in the latter is similar to that in nematic liquids (see Super uid phases of 3 He). BORN APPROXIMATION (M. Born, 1926)

A quantum mechanical perturbation theory method of calculating the probability of scattering of a particle (quasi-particle) off a distancedecaying potential V (r). It is based on using plane waves for both the initial wave function prior to scattering, and the ﬁnal wavefunction far beyond the range of V (r) after scattering. The scattering amplitude in ﬁrst order perturbation theory (ﬁrst Born approximation) is m e−i(k−k )r V (r) d3 x, Akk = − 2 2π where m is the scattered particle mass, and k and k are the wave vectors of the incoming and scattered states of the particle, respectively. Subsequent orders of perturbation theory take into account the deviation of the wave function of the particle from a plane wave, which is caused by the interaction potential. The criterion of the Born approximation is |V (R)| 2 /(mR 2 ), where R is the range of the interaction potential. For an electron scattering off a Coulomb potential, the criterion of the Born approximation is v v (v is the relative velocity of colliding particles, v is the velocity of electron motion in the Bohr

BORON

orbit (see Bohr radius), v = Ze2 /(4πε0 ) (Z is the atomic number, e is the electron charge). The Born approximation ﬁnds wide use in the theory of current-carrier scattering and scattering of other microscopic particles in solids, in the treatment of ionization processes, e.g., light absorption by local electron centers (see Local electronic levels) in nonmetallic crystals, etc. BORN–HABER CYCLE (M. Born, F. Haber, 1919)

A method of approximate determination of the atomic bond energy in crystals (mainly alkalihalide crystals) from experimental data on reaction energies whose sequence (cycle) results in the formation of a crystal from its gaseous atoms. The bonding energy at the temperature of absolute zero is determined as a sum of energies needed for (i) heating the crystal to room temperature (1.5 to 3 kcal/mole); (ii) separating the crystal into the pure metal and the diatomic halide gas (60 to 150 kcal/mole); (iii) sublimation of the metal (20 to 40 kcal/mole); (iv) dissociation of the halogen into a monatomic gas (25 to 30 kcal/mole); (v) cooling the gases to absolute zero (to 2.9 kcal/mole); (vi) removing the valence electrons from alkali atoms (90 to 120 kcal/mole); (vii) formation of negative halide ions from atoms and electrons (70 to 80 kcal/mole). As a result of summing, the bonding energy turns out to equal ∼180 kcal/mole for LiI, ∼185 kcal/mole for NaCl, ∼170 kcal/mole for KCl, ∼160 kcal/mole for KBr, ∼145 kcal/mole for CsI, and so on. Application of methods similar to the Born–Haber cycle allows one to estimate the energies of various reactions in solids, which can be included into one or another cycle, using the known energies of other components of the cycle, e.g., from the energy of formation of Frenkel pairs (see Unstable Frenkel pair) or Schottky pairs in different charge states (see Schottky defect). BORN–VON KÁRMÁN BOUNDARY CONDITIONS (M. Born, Th. von Kármán, 1912)

Periodic boundary conditions imposed on the Bloch function of a particle in a periodic potential, or on a plane wave ϕ(x + Lx , y, z) = ϕ(x, y + Ly , z) = ϕ(x, y, z + Lz ) = ϕ(x, y, z),

127

where Li = Ni ai , i = x, y, z, are the Cartesian coordinates; ai and Ni are the crystal lattice constant and the number of lattice periods in the direction i, respectively. Born–von Kármán boundary conditions allow one to determine the number of allowed states of electrons with different quasiwave vectors k in a unit volume of the reciprocal space. Then, an extra (in addition to the Bloch theorem) condition ψkλ (r + L) = ψkλ (r) (where L is a linear combination of vectors L1 , L2 , and L3 with integer coefﬁcients) is imposed on the wave function. Hence, the number of allowed k values equals the number of unit cells in the volume V = L1 × L2 × L3 and the density of permitted states in k -space equals V /(2π)3 . None of the observed values, including the density of electron states referred to one unit cell, or per unit volume of direct space, are dependent on the selection of L1 , L2 , L3 or V . BORON, B

A chemical element of Group III of the periodic system with atomic number 5 and atomic mass 10.81. The isotope composition of natural boron: 10 B (19.57%) and 11 B (80.43%); the radioactive isotopes 8 B, 12 B and 13 B are known (halflives are fractions of a second). Outer electronic shell conﬁguration is 2s 2 2p1 . Successive ionization energies are 8.298; 25.16 and 37.93 eV. Atomic radius is 0.091 nm; ionic radius of B2+ is 0.023 nm. The most typical oxidation state is +3, and in compounds with metals −3 (borides). In the free state boron exists in the form of brown ﬁne-crystal powder (so-called amorphous boron) and of dark-gray crystals (crystalline boron). The most important boron modiﬁcations are simple α-rhombohedral B (I), tetragonal B (II), and complicated β-rhombohedral B (III). The α-rhombohedral boron lattice parameters are: a = 0.506 nm, α = 58.1◦ , density is 2.365 g/cm3 ; the tetragonal boron lattice parameters are a = 1.012, c = 1.414 nm, and the density is 2.365 g/cm3 ; for β-rhombohedral boron we have: a = 1.014 nm, α = 65.3◦ , density is 2330 kg/m3 . The modiﬁcations B (I) and B (II) under heating above 1773 K irreversibly transform to B (III). T melting of B (III) is 2346 K; T boiling is around 3973 K; thermal coefﬁcient of the linear expansion is

128

BORON CARBIDE

(1.1–8.3)·10−6 K−1 (from 293 to 1023 K). Thermal conductivity coefﬁcient of crystalline boron is 25.96 W·m−1 ·K−1 (at room temperature); speciﬁc heat of amorphous boron is 12.97 J·mole−1 ·K−1 , speciﬁc heat of rhombohedral boron is 11.1 J·mole−1 ·K−1 . Standard enthalpy is 5.895 J·mole−1 ·K−1 for crystalline boron and 6.548 J·mole−1 ·K−1 for amorphous boron; Debye temperature is 1220 K. Crystalline boron is a semiconductor; the forbidden gap width determined from electrical and optical measurements is 1.42 and 1.53 eV, respectively. Boron is a diamagnet, with speciﬁc magnetic susceptibility −0.62·10−9 (at room temperature). It is characterized by high hardness. At low temperatures, boron is a brittle material; above 1800 ◦ C, it begins to deform plastically. Chemically, boron is a nonmetal. Elementary boron has low chemically activity: in the air it burns at 973 K, forming B2 O3 ; with nitrogen above 1473 K, it forms boron nitrides; with carbon above 1573 K, it forms boron carbides. It does not interact directly with hydrogen, but a whole number of hydride compounds Bn Hm is known (see Hydrides), obtained indirectly using silicon. Above 1273 K, there are silicon borides; formed with phosphorus and arsenic above 1173 K are phosphides and arsenides. It ﬁnds wide application in the production of materials (boroplastics), hightemperature strong and superhard materials (e.g., borazon), neutron-adsorbing materials for nuclear power engineering, semiconductor materials, corrosion resistant and antifriction coatings. BORON CARBIDE, B4 C

The only chemical compound of boron with carbon with a broad homogeneity range (molar content of C is 8.6 to 21%). It forms a rhombo5 ), and the hedral lattice of space group R3m (C3v parameters of the crystal lattice in the homogeneity range vary from a = 0.5602 to 0.5616 nm, c = 1.2066 to 1.2120 nm. T melting = 2400 ◦ C, density is 2.51 g/cm3 , thermal conductivity is 121.4 W·m−1 ·K−1 at 300 K, microhardness is 45.0 GPa, elastic modulus is 450 GPa. Boron carbide is a semiconductor of p-type, band gap width is 0.84 eV, electrical resistivity is 0.01 ·m. Boron carbide does not decompose in mineral acids and alkalis. It is obtained through interaction of B2 O3

with coal in arc furnaces, by synthesis from the elements, by crystallization from melts, from their gaseous compounds. Boron carbide is used as an abrasive material, for the borating of metals and alloys, for adsorption of neutrons. BORON NITRIDE, BN

Chemical compound of boron with nitrogen, with three modiﬁcations: α-BN, β-BN, γ -BN. The α-BN compound is hexagonal with space 4 ), crystal lattice paramegroup P 63 /mmc (D6h ters: a = 0.2504 nm, c = 0.6661 nm; β-BN is ¯ cubic with sphalerite-type space group F 43m 2 (Td ), a = 0.3615 nm; γ -BN has the hexagonal wurtzite-like structure, space group P 63 mc 4 ), a = 0.255 nm, c = 0.423 nm. The α-BN (C3v compound transforms into β-BN under high pressure and temperature (P [kbar] = 11.5 + 0.025T ). In the course of heating under normal conditions, β-BN transforms to α-BN at temperatures above 1400 ◦ C; α-BN transforms to γ -BN at shock compression 120 to 130 kbar. The density is 2.20 g/cm3 for α-BN, 3.45 g/cm3 for β-BN and 1.8 g/cm3 for γ -BN; the thermal conductivity is 21 W·m−1 ·K−1 for α-BN and 1800 W·m−1 ·K−1 for β-BN. Microhardness of β-BN is 60 GPa; elastic modulus is 953 GPa. Boron nitride is an insulating material with electrical resistivity ρ > 1015 ·m and band gap width of β-BN ∼10 eV. Boron nitride is obtained by nitration of boron. The α-BN form is used as ﬁreproof and electrical insulating materials; β-BN is a tool and abrasive material. Cubic boron nitride is a superhard material having no natural analogs. It was obtained by Robert H. Wentorf, Gr. (1956) under high pressure (above 4.0 GPa) and temperature (above 1470 K) from hexagonal boron nitride in the presence of alkali and alkali-earth metals, lead, antimony, tin and nitrides of the said metals. The rules of formation of binary compounds with a tetrahedral conﬁguration are as follows. The components should belong to groups equidistant from Group IV of the periodic system; the average number of valence electrons in this compound should equal four. The majority of binary alloys with sphalerite and wurtzite structures satisfy these rules. Cubic boron nitride with sphalerite-type (β-BN) and wurtzite-type (γ -BN) lattices are characterized by

BOSE–EINSTEIN CONDENSATION

the tetrahedral arrangement of atoms with each atom of one type surrounded by four atoms of the other type. In β-BN and γ -BN lattices the four B–N bonds have the same length 0.157 nm, with 109.5◦ angles between them. The crystal lattice of β-BN is similar to that of diamond with spacing 0.3615 nm. Cubic boron nitride is an insulator with a density ≈3.465 g/cm3 . Nanotubes can be made from boron nitride. BORRMAN EFFECT The same as Anomalous passage of X-rays. BORRMAN TRIANGLE (G. Borrman)

A triangle in the scattering plane with one apex lying in the entry surface of a crystal, the two side lines directed along the wave vectors of the incident wave K 0 and the Bragg-diffracted wave K d (see Bragg diffraction), respectively, and the base formed by the segment of the exit surface of the crystal intercepted by these lines. If an X-ray beam is incident along K 0 at a certain point on the entry surface, and the crystal is oriented for Bragg reﬂection, then the wave ﬁeld inside a thin crystal propagates only within the Borrman triangle. Inside a Borrman triangle the response functions also have ﬁnite values (see Dynamic radiation scattering). BOSE CONDENSATE

A macroscopically large number of particles with integer spin (bosons) in an ideal or slightly nonideal Bose gas, which are in their lowest state with zero point energy and momentum at a temperature below the Bose–Einstein condensation temperature. Since the Pauli exclusion principle does not apply, bosons can accumulate in the lowest energy quantum state, all with the same energy forming a coherent condensate. The latter is described by a common complex wave function Ψ = |Ψ |eiΘ with a magnitude |Ψ | and phase Θ that are constant or slowly varying in time. This fundamental property of bosons underlies the phenomena of super uidity in liquid 4 He (see Bose u id) and superconductivity in metals (see Cooper pairs). Related to this is the possibility of laser generation (see Lasers) of a macroscopically large number of photons with the same wavelength under the conditions of a nonequilibrium inverted

129

level population, as well as the possibility of such

an accumulation of photons in a resonator. An analog of a Bose condensate is the ground state in systems with spontaneous symmetry breaking, which is described by a complex order parameter, in particular, the so-called Higgs ﬁeld (see Higgs mechanism). BOSE CONDENSATION The same as Bose–Einstein condensation. BOSE–EINSTEIN CONDENSATION, Bose condensation

The property of Bose particles (bosons) with integer spins to accumulate in macroscopically large amounts in a single quantum state described by a unique (coherent) wave function (see Bose condensate). Bose–Einstein condensation is a property of three-dimensional Bose systems only. It is missing in two- and one-dimensional systems. Bose–Einstein condensation of excitons and biexcitons is a variety this condensation for the case of quasi-particles (excitons and biexcitons, between which repulsion forces dominate). Bose– Einstein condensation of excitons interacting with phonons leads to renormalization of the energy spectrum of both subsystems and alters the shape of light absorption and luminescence bands. The bands contain additional sharp peaks generated by a condensed phase and sloping wings arising from condensate-free excitons. The Fermi nature of electrons and holes forming excitons leads to the non-Boseity of exciton operators. Excitons metallize when their concentration nex becomes −3 of comparable to the inverse of the volume aex the exciton, where aex is its Bohr radius. The Bose–Einstein condensation of excitons is realiz3 < 1 only. able under the condition naex Bose–Einstein condensation of dipole-active excitons and photons (or polaritons with wave vector k0 = 0) is of special interest. In this case, the Bose-condensed state can be considered as an intense coherent wave described by a coherent Glauber state with a macroscopic amplitude. Equations describing inhomogeneous in space and time weakly of excitons and of photons have been derived; the diagram techniques for nonequilibrium states has been developed to describe coherent quasi-particles existing simultaneously with

130

BOSE–EINSTEIN STATISTICS

a condensate. On this basis, the features of coherent nonlinear propagation of light in densely condensed media are assigned to the exciton spectral range. The values of wave vectors and frequencies have been found, where, due to the absolute and convective instability of the spectrum, generation and ampliﬁcation of waves is possible. Rearrangement of the energy spectrum of the phonoriton type (see Phonoriton) is due to peculiarities of the distribution functions of incoherent quasi-particles and conditions of stimulated Brillouin scattering of light. The role of quantum ﬂuctuations and the inﬂuence of incoherent polaritons upon the statistical properties of an intense polariton wave have been clariﬁed. A stimulated Bose– Einstein condensation of excitons and polaritons under the action of coherent resonant laser radiation, and a stimulated Bose–Einstein condensation of biexcitons obtained by two-photon excitation with counter-directed or parallel laser beams, were experimentally carried out. BOSE–EINSTEIN STATISTICS (Sh. Bose, A. Einstein, 1924)

The statistics describing the distribution in quantum states of a system of very many identical particles with zero or integer (in units) spin. Particles as well as quasi-particles that obey Bose–Einstein statistics are called bosons; including photons, phonons, magnons, excitons, bipolarons, π -mesons, and so on. The wave function of bosons is symmetric with respect to the exchange of any pair of particles. A particular feature of bosons is the possibility for any number of them to be in the same quantum state. In view of this property, it follows from the Gibbs distribution that the average number of particles ni in quantum state i with energy εi for a boson ideal gas (Bose gas) in thermodynamic equilibrium is −1 εi − μ −1 ni = exp , (1) kB T where k B is the Boltzmann constant, μ is the chemical potential determined by the total

number N of particles in the system, and N = i ni (μ). In a system with a variable number of particles, μ = 0; under constant N , μ < 0. Eq. (1) is called the Bose–Einstein distribution. At low temperatures, a ﬁnite portion of the particles pass to

the lowest states with ε = 0; their number N0 = N[1 − (T /T0 )3/2 ] where N 2/3 2 3.31 T0 ∼ = gV mk is called the condensation temperature, g is the degeneracy factor, m is the particle mass, V is the system volume. Other particles are distributed over states according to Eq. (1) at μ = 0. Such a transition is called a Bose–Einstein condensation (Bose condensation). The Bose–Einstein distribution determines the efﬁciency of scattering of particles moving in a solid (electrons and holes, neutrons, photons etc.) by photons, nonradiative quantum transitions in solids, phonon–phonon interactions and also values of electrical conductivity and thermal conductivity, speci c heat, acoustical properties, parameters of optical bands, spectral composition of black body radiation, and so on. BOSE FLUID A quantum liquid that condenses at low tem-

peratures and consists of interacting bosons, i.e. particles with integer (in units) intrinsic angular momentum (spin). An example of a Bose ﬂuid is liquid helium (4 He) at T < 4.2 K. Below some critical temperature (see Lambda point) Bose ﬂuids can transform into the superﬂuid state (see Super u idity). BOSE GAS (Sh. Bose)

A quantum system of weakly interacting particles (quasi-particles) with integer spins (bosons) subject to Bose–Einstein statistics with the distribution function (at spin σ = 0) −1 ε −μ −1 , nk = exp k kB T where εk is the energy of the kth quantum state or of a free particle with momentum k, μ is the chemical potential (μ 0), T is the absolute temperature. A Bose gas of neutral particles is ideal for a small density n, when n1/3 r0 1, where r0 denotes the action radius of exchange or van der Waals forces, and a Bose gas of electrically charged bosons (e.g., bipolarons) becomes weakly nonideal at a high density, when n1/3 a0 1, where a0 denotes the Bohr radius of particles. In

BOUNDARY EFFECTS

a Bose gas with a given (constant) number of particles, under a pronounced decrease of temperature, Bose–Einstein condensation takes place, while in a Bose gas with a variable number of particles (quasi-particles) determined by the thermodynamical (thermal) equilibrium condition (e.g., the phonon gas in a crystal or in liquid helium), the Bose–Einstein condensation does not occur. BOSE STATISTICS The same as Bose–Einstein statistics. BOTTLENECK OF PHONONS See Phonon bottleneck. BOUNDARY DIFFUSION Diffusion over two-dimensional structural defects like grain boundaries and subgrains, i.e. over

elements of imperfection of the crystal structure which separate parts of a bulk metal from crystal lattices of different space orientation, different crystal structure, or different material composition. Among the various types of boundary diffusion, the greatest interest involves material transfer over grain boundaries in polycrystalline materials. Boundary diffusion deviates from the usual Arrhenius linear dependence (see Interdiffusion) of log D versus 1/T where D is the diffusion coef cient; lower temperatures and grain pulverization result in greater departures from the Arrhenius law. The boundary diffusion coefﬁcient in metals is usually several orders of magnitude higher than that for bulk diffusion. A model for quantitatively estimating diffusion parameters put forward by I.C. Fisher (1951) provides the expression 0.21(D/t)1/2 , tan2 α where D GB is the diffusion coefﬁcient over the grain boundaries, t is the diffusion time, δ is the width of the boundary layer, and α is the slope of the straight line characterizing the dependence of the logarithm of the concentration on the diffusion depth. According to various authors the width of the boundary layer lies in the range from 0.3 nm to a few μm. The boundary layer has a so-called diffusion width, i.e. a region in which the mobility of atoms is higher than in the bulk. This width is approximately double the distance from DGB δ =

131

the grain boundary to the point where the diffusing atom concentration is reduced by the factor of e = 2.718 from its maximum value. For some metals (e.g., for self-diffusion in nickel) this distance is 4 to 5 μm. Diffusion over a phase boundary is of great importance for phase transition kinetics. On a phase boundary, like on a grain boundary, a change of the crystal lattice state, defect clustering, and chemical segregation are possible factors that enhance the atomic mobility compared to that in the bulk. The principal methods for investigating grain diffusion are macro-, micro- and electron microscopic autoradiography, and the method of secondary ion–ion emission. BOUNDARY EFFECTS in liquid crystals

Effects caused by the action of anisotropic surface forces. In technological applications and in laboratory studies liquid crystals are in contact with substrates and hosts (glass, polymers, isotropic liquids, cleavages of monocrystals, and so on). Anisotropic interphase interactions caused by the mutual action of various molecular forces (dispersion, dipole–dipole, steric) orient the molecules of a liquid crystal either normal to the boundary (homeotropic orientation), at an angle (conical or tilted orientation), or in the plane of the boundary (planar orientation). A quantitative measure of the orienting action of the substrate (i.e. of the external medium) on the liquid crystal is the cohesion energy (anchoring energy) W . The magnitude of W determines the work needed to turn the director (molecules) of the liquid crystal from its equilibrium position at the boundary through a certain angle. If W is comparable to or greater than the energy of intermolecular interactions in the liquid crystal then the cohesion is called strong; otherwise it is called weak. Owing to long-range orientational ordering (see Orientational order), the conditions of cohesion at the surface affect the bulk properties of the liquid crystal. For example, in the case of weak cohesion the threshold tension of a Frederiks transition is reduced; at the same time, the response time decreases with a simultaneous increase in the steepness of the voltage–contrast characteristic in a liquid crystal cell, and this allows one to increase the information capacity of liquid-crystal displays. Boundary effects inﬂuence not only in the type of orientation of the molecules

132

BOUND WATER

on the surface, but also the degree of order in the interior. Near the surface the degree of order differs from that in the bulk (the former being higher, as a rule). It is experimentally possible to form, at the boundary of a nematic liquid crystal, a thin layer of smectic liquid crystal that is characterized by extra translational ordering of the molecules, and by a higher degree of orientational ordering of their long axes. The spatial inhomogeneity of the degree of ordering near the liquid crystal surface results in a macroscopic electric polarization of the subsurface layer which is referred to as order electricity (compare with the exoelectric effect). BOUND WATER, combined water

Water interacting with the surface of mineral particles, and thereby acquiring some special properties. It freezes at temperatures below 0 ◦ C. The “bonding” mechanism of water in rocks involves the processes of physical and chemical adsorption, capillary condensation (see Capillary phenomena), and osmosis. The action of surface forces in minerals results in the perturbation of hydrogen bonds between the molecules of water, which is then transferred in succession from molecule to molecule of water. Bound water is usually separated into adsorbed, capillary, and osmotic types. Adsorbed water is more strongly held at the surface of minerals, and is therefore considered strongly bound, while capillary and osmotic water are both weakly bound. Strongly bound water is nonuniform. One may identify “island” water adsorption (bonding energy within 40–130 kJ/mol) and multilayer adsorption (bonding energy within 0.4–40 kJ/mol). Capillary and osmotic water are contained in rocks at humidities exceeding the maximum rock hygroscopicity. They both differ in their properties from either free or strongly bound water. Osmotic water may only be contained in rocks if some ions are present. It is the type most weakly bound to the surface, with its bonding energy remaining below 0.4 kJ/mol. The freezing temperature for capillary and osmotic water varies from −0.2 to −(2–3) ◦ C. BOUSSINESQ EQUATION (J. Boussinesq, 1871)

An equation of the form Ut t − Uxx − 6(U 2 )xx − Uxxxx = 0, where U (x, t) is the velocity ﬁeld; and x and t are, respectively, the space

and time coordinates written in a dimensionless form (subscripts denote partial differentiation). This equation was introduced by Boussinesq to describe the propagation of waves of small but ﬁnite amplitude when the dissipation is negligible, and characteristic wavelengths signiﬁcantly exceed the reservoir depth. In solid-state physics, the Boussinesq equation is also referred to as a nonlinear string equation in connection with its application to the theory of nonlinear waves of a one-dimensional lattice and a nonlinear string. The Boussinesq equation is more general than the Korteweg–de Vries equation (see Soliton) because it takes into account motion in both directions. The Boussinesq equation is completely integrable by the inverse spectral transformation associated with a scattering problem for a third order operator. Therefore, it has all attributes pertinent for integrable systems: an inﬁnite series of polynomial conservation laws, Bäcklund transformation, and many-soliton solutions. The simplest singlesoliton solution of the Boussinesq equation is x ± ct 1 2 2 , U (x, t) = c − 1 Sech 4 Δ where c is the soliton velocity, and Δ = 2(c2 − 1)−1/2 is its width. It is a single parameter family of stationary solitary waves. There are several modiﬁcations of the Boussinesq equations which cannot be integrated. In particular, Ut t − Uxx − 6(U 2 )xx − Uxxt t = 0 is the adjusted Boussinesq equation used to describe longitudinal acoustic waves in rods; and Ut t − Uxx − 6(U 3 )xx − Uxxt t = 0 is the modiﬁed adjusted Boussinesq equation used in the theory of nonlinear seismic waves. BOUSSINESQ–GALYORKIN SOLUTION (J. Boussinesq, B.G. Galyorkin)

A general solution of the equilibrium equations of an elastic medium in the absence of bulk forces expressed via an arbitrary biharmonic vector. If the equilibrium equation is written in the form (1 − 2ν)∇ 2 u + grad div u = 0, where u is the displacement vector, and ν is the Poisson ratio, then the Boussinesq–Galyorkin solution has the form: 1 (1 − ν) × grad div f , u = ∇2f − 2

BRAGG MULTIPLE SCATTERING

where f is an arbitrary biharmonic vector, i.e. a vector satisfying the equation ∇ 2 ∇ 2 f = 0. BRAGG DIFFRACTION (W.L. Bragg)

A type of diffraction of X-rays, neutrons, electrons, etc., by crystals when the reﬂection from each plane of atoms is specular, and the rays reﬂected from successive planes constructively interfere with each other. Symmetric and asymmetric Bragg diffraction are distinguished in which the reﬂecting planes (hkl) are parallel or not parallel to the entrance plane of the crystal, respectively. The most important effect in Bragg diffraction is the total interference reﬂection of the transmitted wave in a small angular interval (for X-rays, a few seconds of arc) due to the extinction effect when the wave ﬁeld penetrates a crystal to a depth of the order of the extinction length. The reﬂectivity of a crystal of ﬁnite thickness in Bragg diffraction has some subsidiary maxima in its angular dependence, which are the analogues of the pendulum solution in Laue diffraction. Bragg diffraction is mostly employed to check the structural perfection of the near-surface layers of crystals. Unlike Laue diffraction, Bragg diffraction is not limited by sample thickness t ; and for thick samples t tn , where tn is the absorption length, the diffraction pattern is simpler, and it is more readily interpreted. BRAGG DOUBLE REFLECTIONS

This diffraction occurs when an X-ray, electron, neutron, etc., beam reﬂected in accordance with the Bragg law from a family of parallel planes in a crystal reﬂects again from the planes of the same family. The direction of propagation and the intensity of Bragg double reﬂections are determined by the crystal structure of a crystal, and by the experimental conditions. While the ﬁrst and the second reﬂections occur in crystal regions disoriented by the angle δ, the direction of Bragg double reﬂections differs from that of the primary radiation by the angle ε = δ sin θ where θ is the Bragg angle. There are three kinds of Bragg double reﬂections in polycrystals: intrablock, intragrain and intergrain ones. At large scattering angles (ε 10◦ ), these reﬂections are veiled by the diffuse background due to Compton scattering (see Compton

133

effect) and thermal scattering. At small scattering angles (ε 1◦ ), the contribution of Bragg double reﬂections is signiﬁcant and exceeds the thermal and the Compton scattering by several orders of magnitude. The small-angle scattering of X-rays due to Bragg double reﬂection allows one to determine the size of grains and blocks in polycrystals, their orientation distribution, and the angular block disorientation (see Bragg multiple scattering). BRAGG LAW, Bragg relation (W.H. Bragg, W.L. Bragg, G.V. Vulf, 1913) The main equation of X-ray diffraction. X-ray

diffraction from the atomic lattice of a monocrystal can be formally described as reﬂection from atomic planes. According to the Bragg law, the angle of reﬂection (Bragg angle) θ between the atomic plane and diffracted beam satisﬁes the condition 2dhkl sin θ = nλ, where dhkl is the interplane distance between the series of parallel atomic planes with crystallographic indices (hkl), λ is the X-ray wavelength, and n = 1, 2, 3, . . . is the order of the reﬂection. BRAGG MULTIPLE SCATTERING Scattering of radiation in a crystal under the conditions when the Bragg relation (see Bragg law) is valid for two or n reﬂections simultane-

ously. One can represent the conditions of the Bragg multiple scattering with the help of an Ewald sphere in k -space: the Ewald sphere with radius |k 0 | = 1/λ corresponds to the incident radiation with wavelength λ. Vectors k 0 , k 1 , k 2 corresponding to the incident wave and waves reﬂected from reciprocal lattice sites (1) and (2) for the case of triple Bragg scattering are shown in the ﬁgure (n = 3, including the primary beam). Here, |k 0 | = |k 1 | = |k 2 |. By rotating the crystal about the scattering vector (straight line H01 connecting sites (0) and (1)), one can remove site (2) from the Ewald sphere, i.e. violate the Bragg condition for the site and thus exclude the triple dynamic scattering. At this, site (1) remains at the sphere and the Bragg condition applies to it (see Bragg double re ections). The greater the dimensions of a crystal unit cell and the shorter the wavelength λ (i.e. the larger the Ewald sphere radius),

134

BRAGG RULE

BRAKING RADIATION See Bremsstrahlung. BRANCHING OF FRACTURES

Bragg multiple scattering.

the greater the number of reciprocal lattice sites that can be on the sphere. That is, the more difﬁcult it will be to ﬁnd a position of the crystal where there is no Bragg multiple scattering. The evaluation of the contribution of the Bragg multiple scattering to the intensity of the measured reﬂection is quite a difﬁcult problem to solve, considering that it is complicated by the crystal mosaicity, the divergence, and the nonmonochromaticity of the incident radiation. Bragg multiple scattering allows one to observe reﬂections in those directions where the Bragg scattering is prohibited by the crystal symmetry conditions; this is the so-called Renninger effect (M. Renninger, 1937). Bragg multiple scattering in crystals can also play a positive role, e.g., it underlies one of the methods of high-precision determination of crystal lattice parameters. BRAGG RULE

This rule involves charged particle energy loss during the passage through a material with the chemical formula Al Bm Cn . . . and it is expressed by the approximate relation dE dE dE +m − =l − − dZ dZ A dZ B dE +n − + ···, dZ C where (−dE/dZ)i , i = A, B, C, are the energy losses per unit length due to the ith component of the material.

A process of the separation (bifurcation or polyfurcation) of a main-line fracture into two or more secondary ones. One can distinguish quasistatic branching of fractures caused, in particular, by processes of plastic deformation at its vertex, and dynamic branching which is observed when the fracture attains about 60% of the speed of transverse elastic waves. Due to this the stresses in front of the fast moving fracture stop being a maximum, and the failure becomes more probable in other directions. Dynamic branching of fractures has been observed in hardened glasses (see Vitreous state of matter), steels, Plexiglas and epoxy resins. Branching arises in the core layers of a sample at the front of the main-line fracture, and is directed along the tangent to the curved segment of the fracture trajectory. Thus, a secondary fracture is oriented at an angle of approximately 30◦ with respect to the primary one. After each act of branching the speed of the main-line fracture decreases. Therefore, multiple branching produces destructions that move in jumps with high accelerations, up to 108 m/s2 , thus managing to branch at small distances (e.g., in the millimeter range for hardened steel), break loose, pick up critical speed, and then branch again. The branching is stimulated by internal residual stresses that arise in the sample being fractured. BRASS

Alloy of copper and zinc belonging to the class of compounds with metallic bonding. It exists over a wide range of concentration. At low Zn content the alpha phase (face-centered cubic lattice) is formed. At higher Zn content the stability of the new phases (the so-called “electronic phases”) is determined by the average concentration n of valence electrons per atom via the proper matching of the Fermi surface and the Brillouin zone. The three electronic phases are the beta phase (compound CuZn, body-centered lattice, n = 3/2, below 460 ◦ C ordered according to the CsCl type), gamma phase (compound Cu3 Zn8 , complex cubic lattice, ordered, contains 52 atoms, n = 21/13) and epsilon phase (compound CuZn3 , hexagonal

BREAKDOWN

135

Brass phase diagram.

close-packed lattice, n = 7/4). Unusual mechanical properties are found in β-brass, caused by a martensitic transformation (shape memory effect, superelasticity, high damping). The ﬁgure shows the phase diagram. BRAVAIS LATTICES (A. Bravais, 1848)

The classiﬁcation of three-dimensional lattices into 14 types that takes into account the full point symmetry groups (holohedries) and the parallel translation groups. If a Bravais coordinate system (chosen along the most symmetrical directions of the lattice) coincides with the principal lattice system then the Bravais parallelepiped constructed on it contains lattice sites only at its apices, i.e. is a primitive parallelepiped. Such lattices are called primitive or P lattices; all other lattices are referred to as centered lattices. There are three ways to center the Bravais parallelepipeds, I – body-centered, F – facecentered, and C – base (or side)-centered. Two lat-

tices are included in the same Bravais type if their coordinates are the same and the parallelepipeds are centered identically. The Bravais classiﬁcation has also a group theory basis: two lattices are included in the same Bravais type if their full symmetry groups are isomorphous (see Isomorphism). These groups (14 out of 73 symmorphic space groups) are called Bravais groups and are designated by the symbols of the space groups. Each of 14 Bravais types is presented in Table 1 (see next page) by a corresponding Bravais parallelepiped with points at the apices, and where appropriate, with centering points indicated (see inside front cover). BREAKDOWN of solids

A sharp increase of electric current density in insulators and semiconductors that occurs when a

certain critical level of the applied electric ﬁeld strength, Ecrit , is reached. The value Ecrit is called the electric strength. The value of Ecrit falls within

136

BREAKDOWN Table 1. Bravais lattices Lattice type System

Primitive

Base-centered

Body-centered

Face-centered

Triclinic

Monoclinic

Orthorhombic

Trigonal (rhombohedral)

Tetragonal

Hexagonal

Cubic

105 –107 V/cm for various dielectrics and starts from 105 V/cm for semiconductors. During impact ionization it may be as low as 1 to 10 V/cm. One may distinguish between the electric and thermal mechanisms of breakdown. The mechanism of electric breakdown is typically characterized by an avalanche increase of the number of free carriers (electrons or electron–hole pairs), for example due to ionization by collision. Current lamentation may also occur, i.e. a conducting channel in which the current density is higher than its average across the sample may form. This effect results from an instability of the spatially homogeneous distribution of carriers when the sample

current–voltage characteristic has an S-shape. In

the case of an electric breakdown the value of Ecrit only weakly depends on the sample temperature, thickness, and the duration of electric ﬁeld pulse, τ , provided τ = 10−7 –10−6 s. Thermal breakdown results from melting of the material via Joule heating when its thermal equilibrium is disturbed (thermal breakdown without a disturbance of thermal equilibrium is also known, the so-called type II thermal breakdown). A combined mechanism of breakdown is possible, when the Joule heating of a particular region of the sample works to lower the value of Ecrit necessary for an electrical breakdown in that region. The application of a strong

BREMSSTRAHLUNG

137

ﬁeld may result in a gradual change of the composition and structure of an insulator, so that both eventually work to lower the value of Ecrit . These effects could, for example, lead to the formation of color centers in alkali-halide crystals or to erosion of polymer surfaces. Such processes are called electric aging of insulators. In contrast, dielectric breakdown in semiconductors may not necessarily be accompanied by changes in the crystal lattice. In certain cases, when the conduction electron concentration is limited and the ﬁeld strength, E is moderate, the initial process of breakdown does not result in the failure of the material, and may be repeatedly reproduced (see Impurity breakdown, Thermoelectric instability of photocurrent, Streamer breakdown). For different varieties, see also Acoustic breakdown, Electric breakdown, Magnetic breakdown.

more parts. Breaking stress is deﬁned by the ratio of the load to the specimen cross-section at the moment of failure. In brittle metals (see Alloy brittleness) this stress is achieved via the opening of brittle cracks when the external stress remains below the yield limit, and macroscopic plastic deformation is absent. When plastic metals subjected to stresses exceed the yield limit, there develops a tough failure or a quasi-brittle failure in them, while the failure stress exceeds the yield limit because of strain hardening. Failure stress in brittle metals depends only weakly on the temperature, approximately as the elastic modulus, while its dependence in plastic materials is controlled mainly by the temperature dependence of the yield limit, and may happen to be stronger.

BREAKDOWN NOISE See Telegraph noise.

An exact solution of the secular equation for the spin Hamiltonian of a paramagnetic ion with electron effective spin S = 1/2, nuclear spin I , and isotropic g, g n and hyperﬁne (A) tensors. The energy levels are as follows:

BREAKING STRAIN Strain that results in the break-up of a body into several macroscopic parts (failure). The break-

ing strain produces such a degree of deformation that it results in failure. This strain is one of the principal characteristics of a material, delimiting its margin of plasticity. It is determined during the mechanical testing of materials. Breaking strain depends on the type of state of stress (distension, compression, e xure etc.), i.e. on the “rigidity” of various types of mechanical n , tests, and on the softness factor a = tmax /Smax which is the ratio of the maximum tangential tension, tmax to the maximum normal reduced stress, n . With an increase in the material capabilSmax ity to withstand stress the plastic deformation increases. Breaking strain also depends on the type of crystal lattice, the structure, testing temperature, environment, etc. When determining the level of breaking strain the scheme reproducing both the tensed and the deformed states of the specimen during tests should be as close as possible to the actual operating conditions of the material. BREAKING STRESS, failure stress, failing stress

A stress reached during distension tests, which result in the breakup of the specimen into two or

BREIT–RABI FORMULA (G. Breit, I. Rabi)

Δ − gn βn BmF 2(2I + 1) 1 4xmF 1/2 ± Δ 1 + x2 + , 2 2I + 1

E(F, mF ) = −

where F = I + 1/2, mF = m ± 1/2, m = −I, . . . , +I ; Δ = a(I + 1/2) is the splitting in zero magnetic ﬁeld B; a is the isotropic hyper ne interaction constant, x = (gβ + gn βn )B/Δ, and β and βn are the Bohr and nuclear magnetons, respectively. BREMSSTRAHLUNG, braking radiation, collision radiation

An emission of photons by electrically charged particles decelerating in an electric ﬁeld (or in a magnetic ﬁeld, called magnetic Bremsstrahlung or synchrotron radiation). The intensity of Bremsstrahlung is proportional to the square of the particle acceleration, i.e. proportional to Z 2 /M 2 where Z is the atomic number, and M is the mass of the nucleus being decelerated by the electric ﬁeld. Owing to the small mass of elec-

138

BREMSSTRAHLUNG, COHERENT

trons and positrons, the intensity of their Bremsstrahlung is 3·106 times greater than that for protons. This leads to a substantial contribution to the Bremsstrahlung by the energy loss of fast electrons and positrons in a medium (see Charged particle energy loss). The spectrum of Bremsstrahlung is continuous. The maximum value of the energy of the emitted photon is ωM = E − mc2 (here E is the total energy, m is the electron mass, and c is the speed of light). In a crystal the constructive interference of photons scattered by closely situated atoms of the crystal inﬂuences some speciﬁc features of the Bremsstrahlung, in particular the intensity of the Bremsstrahlung increases (see Coherent Bremsstrahlung). These changes are especially signiﬁcant in the case of the channeling of electrons and positrons (see Quasi-characteristic radiation). See also Radiation by charged particles. BREMSSTRAHLUNG, COHERENT

See Coherent Bremsstrahlung. BRILLOUIN FUNCTION (L. Brillouin, 1926)

Function Bj (x) introduced to describe paramagnetism of noninteracting atoms. For atoms with the angular momentum j (in units of Planck constant ), the function is Bj (x) =

2j + 1 2j + 1 coth x 2j 2j −

1 x . coth 2j 2j

The Brillouin function determines the mean value of the projection of j on the direction of the magnetic ﬁeld H (directed along the z axis) jz = j Bj (x), x = gj |μB |H /(k B T ), where μB is the Bohr magneton and gj is the Landé g -factor. The Brillouin function is the basis for the quantum theory of paramagnetism of substances with uncompensated atomic magnetic moments, and of magnetically ordered materials (when described in the framework of the molecular eld approximation; in this case, H is the effective magnetic ﬁeld).

BRILLOUIN SCATTERING, also called Mandelshtam–Brillouin scattering Inelastic light scattering by thermal acoustic phonons in condensed media with the light fre-

quency changed by a value equal to a phonon frequency. (Analogous processes by optical phonons are called Raman scattering of light). The scattering is caused by ﬂuctuating inhomogeneities of the refractive index, which are related to propagation of thermal (Debye) excitations of a medium. From the classical point of view, Brillouin scattering can be interpreted as result of the diffraction of light by thermal elastic waves. By virtue of the diffracted light interference, only waves with wavelength Λ, which satisﬁes the Bragg condition λl = 2nΛ sin(θ/2) (where n is the refractive index of the medium, λl is wavelength in vacuum, θ is angle of scattering), are responsible for scattering in a given direction. Furthermore, due to the Doppler effect, the light with frequency ωl , which is scattered by elastic waves, undergoes a frequency change ωs = ωl ± ω0 , deﬁned by the relationship ω0 /ωl = ±v/(Λωl ) = ±2n(v/c) sin(θ/2), where c is the speed of light in vacuo, and v is the sound velocity in the medium. Elastic waves with frequency ∼1010 Hz (hypersonic waves) are of importance in the light scattering. The line width is determined by hypersound attenuation. The scattering efﬁciency is of the order of 10−6 scattered photons per incident photon. However, if the intensity of the incident light exceeds some threshold value (∼1010 W/cm2 ), an avalanche-like growth of the amplitudes of sound and of scattered waves occurs, a process called stimulated Brillouin scattering. Brillouin scattering is used for studying material properties: sound wave propagation velocity and decay rate, molecular structure, intermolecular interactions, etc. Stimulated Brillouin scattering is used for the generation of intense hypersonic waves, and in experiments on wave front reversal of light waves. Resonance Brillouin scattering is an effective method for investigating excitonic polaritons. BRILLOUIN ZONE

A limited region in the reciprocal space (k -space) of wave vectors inside which the quasiparticle energies in the crystal take on the entire

BRITTLE FRACTURE

spectrum of permitted values. The overall k-space can be partitioned into an inﬁnite number of Brillouin zones of the same dimensions, and equal in volume to a reciprocal lattice cell. The use of a single Brillouin zone is due to the crystal periodicity since the quasi-particle energy E(k) is periodic in the quasi-momentum space with the periodicity of a reciprocal lattice vector G: E(k) = E(k + G). A region with its center at the point k = 0 is chosen as the ﬁrst Brillouin zone, or simply referred to as the Brillouin zone. It is delimited by planes passing through the mid-points of the lines (normally to them) that connect point k = 0 with neighboring sites of the reciprocal lattice. A Brillouin zone is analogous to a Wigner–Seitz cell in real (coordinate) space. Its boundaries are determined by the reciprocal space form of the Bragg equation 2k·G = G2 , involving a reciprocal lattice vector. At the boundaries the quasi-particle energy E(k) reaches an extremum. To describe some physical phenomena it is convenient to use the extended Brillouin zone scheme which makes use of the periodicity of the quasi-particle spectrum in k-space. BRITTLE CRACK A crack, whose propagation is not followed by a plastic deformation. During brittle crack propagation the theoretical strength is reached at its

vertex. The breaking of interatomic bonds occurs without activation. Elastic energy, stored in the material during a deformation process, converts into surface energy at its propagation. The critical stress for the brittle crack propagation is determined by the Grifﬁth equation (see Grif th theory). BRITTLE FAILURE

A type of solid failure involving purely elastic strains. Ideally only materials with no capability for plastic deformation (e.g., glass, ceramics, diamonds, some minerals) undergo brittle failure under conditions of ordinary tension. Metals, due to the presence of dislocations, behave as ideally brittle only in special circumstances when the failure is initiated in extremely small regions. These regions have an ideal (defect free) structure in perfect crystals (whiskers), or in microregions near the tip of atomically-sharp submicrocracks,

139

where a fracture of atomic bonds occurs through microspalling (without attendant plastic deformation). However, in so far as the origin of microcracks in metals is possible only as a result of the displacement and pile-up of dislocations, so a failure in metallic materials can only be of a quasibrittle type (see Quasi-brittle failure) since a condition of purely elastic deformation does not appear at their failure. In practice when a failure of products, constructions and installations (e.g., hulls of ships) occurs, it is considered to be the brittle type, if an overall deformation of the product was elastic before its failure, in spite of the fact that a large local plastic deformation took place in the focus of failure. Hence in practice the term “brittle failure” does not have a precise meaning. However, it can correspond to a complicated type of failure combining features of overall elastic and local plastic deformation. The latter forms only in small regions near cracks, or in action zones of large residual stresses of a welding or quenching origin. An important feature of such a failure is that the average (nominal) failure stress should be less than the yield limit of the material. Excessively high strength of the material, low temperature (cold brittleness), high velocity of deforming (a shock load), the presence of cracks or other concentrators of stresses, the presence of large residual macrostresses of the ﬁrst type; all of these factors contribute to the signiﬁcance of brittleness in engineering practice. BRITTLE FRACTURE A fracture arising from brittle failure. This type of failure is associated with failure by spalling,

when a progression of the crack is not accompanied by plastic deformation, and failure occurs over the plane of crystal cleavage through the breaking of atomic bonds. Actual brittle failure has been found in covalent crystals such as diamond and silicon carbide. A brittle transcrystalline failure is possible also in other crystals with a high degree of covalent bonding, where dislocations are practically “frozen in”. The typical feature appearing on the surface of a brittle fracture is a step of spalling arising at the intersection of a screw dislocation and a crack front. A junction of the splitting steps makes up a stream-like pattern. The same

140

BRITTLENESS AND TOUGHNESS CRITERION

features of fracture are typical for quasi-brittle failure through splitting accompanied by plastic deformation of the region adjacent to the crack. Such a failure is typical for crystals with body centered cubic lattices at ambient temperatures. Intercrystalline brittle failure occurs at sharply weakened intergranular linkages. It is observed along grain boundaries through the catastrophic crack progress due to the segregation of impurities, and also to the presence of internal stresses. Intercrystalline failures along boundaries of grains and subgrains are distinguished. When a failure runs along grain boundaries a fracture is completely free from a stream-like pattern, linkage points of three (or more) boundaries of grains appear, and often a “bubble” due to the segregation of impurities is observed on facets of split grains.

the failure is supposed to be tough. In mechanics, the engineering criterion of brittleness is used, whether the product is destroyed by the average (nominal) stress σn below the yield limit σy , i.e. when σn < σy , which can be satisﬁed only in the presence of stress concentrators (see Stress concentration). BRITTLENESS, BLUE See Blue brittleness. BRITTLENESS OF ALLOYS See Alloy brittleness. BROADENING OF A LINE See Line (level) width. BROKEN BOND The same as Dangling bond.

BRITTLENESS AND TOUGHNESS CRITERION

This is a condition determining the relation of parameters responsible for the type of failure of a solid under load. There is no unique brittleness and toughness criterion, since these criteria differ in various areas of science involving failure problems. In solid state physics, the brittleness and toughness criterion is connected with the possibility of plastic stress relaxation via the generation of dislocations by a vertex of a perfectly sharp crack in a crystal. This possibility depends on the relation between theoretical strength against shear τtheor and rupture σtheor and maximum tangential τmax and tensile stress σmax at the vertex of the crack. If τtheor /σtheor < τmax /σmax , the crystal is tough (FCC metals: copper, silver, gold); otherwise, it is brittle (diamond and BCC metals: tungsten, iron, sodium). In physical materials science, as a brittleness and toughness criterion, the one based on the microspalling criterion my be chosen: if j > Kt , then the failure is brittle, if j < Kt , then it is tough (more precisely, a quasibrittle failure). According to the fractographic classiﬁcation of destruction types, one does not succeed in giving a clear distinction between brittleness and toughness in metals, and brittleness and toughness criteria are qualitative: if in a fracture of brilliant facets of a spalling no appreciable traces of plastic deformation are seen, then the failure is supposed to be of a brittle (or quasi-brittle) type; if typical pores or pits are observed (a ﬁbrous break),

BROOKS–HERRING FORMULA (H. Brooks, C. Herring)

This expression determines the energy dependence of the mean free path time τ (E) of charge carriers of energy E in semiconductors when the scattering takes place predominantly from ionized impurities (low temperatures, high impurity concentrations). The Brooks–Herring formula is τ (E) =

ε2 (2m∗ E 3 )1/2 , πe4 NΦ(x)

where ε is the dimensionless dielectric constant; m∗ is the effective mass of the carriers, N is the impurity concentration, Φ(x) = ln(1 + x) − x/(1 + x) where x = 8m∗ E/(2 q 2 ), q is the inverse Debye screening radius. It follows from the Brooks–Herring formula that scattering by ionized impurities becomes more efﬁcient at small carrier energies and, consequently, at low temperatures. The Brooks–Herring formula was derived in the Born approximation of collision theory taking into account the screening of impurities by free carriers. In its derivation the impurities are assumed to be arranged in a crystal lattice in a disordered way (see Current carrier scattering). BUBBLE DOMAIN See Magnetic bubble domain. BUBBLE DOMAIN LATTICE See Magnetic bubble domain lattice.

BULK PHOTOVOLTAIC EFFECT

BUCKYBALL See Fullerene. BULK ACOUSTIC WAVES Propagating periodic strains of an elastic me-

dium obeying the wave equation ρ∂ 2 ui /∂t 2 − cij kl ∂ 2 uk /∂xj ∂xl = fi , where ρ is the medium density, u is the displacement of the medium element, cij kl are the components of the elastic modulus tensor, and f is the bulk density of the external (nonelastic) forces. In contrast to liquids and gases, solids can support the propagation of traverse waves in addition to longitudinal waves; the displacements in the former being normal to the propagation direction. Three natural modes of acoustic waves exist in an isotropic body (see Isotropy): one longitudinal acoustic wave with the velocity v = (c1111 /ρ)1/2 , and two degenerate transverse acoustic waves with v⊥ = (c1212 /ρ)1/2 . In an anisotropic medium (such as a crystal) pure longitudinal and traverse waves can propagate only in preferred directions which have sufﬁciently high symmetry. For an arbitrary propagation direction, there are three modes of bulk waves with different phase velocities (a typical sound velocity in solids is v ≈ 105 cm/s). Acoustic waves can be classiﬁed by their frequency. Waves in the audible and infrasonic range (f < 104 Hz) lack important applications in solid state physics due to their long wavelength. Waves with frequencies from 20 kHz to 1 GHz are called ultrasonic (ultrasound), and are widely used in physics and engineering. The frequency range 109 to 1012 Hz, called hypersonic (hypersound), exhibits quite sizable attenuation (attenuation coefﬁcient κ > 1 cm−1 ). Acoustic waves with frequencies above 1012 Hz are called terasound, and exhibit a signiﬁcant dispersion as their wavelength becomes comparable to the crystal lattice period. Sound velocity dispersion and anisotropy of the medium cause the group velocity characterizing the propagation of perturbation waves, which has a narrow spectral-angular distribution (v gr = ∂ω/∂k), to differ from the phase velocity describing the phase propagation (v ph = kω/k 2 ) in both magnitude and direction. BULK CHARGE The same as Space charge.

141

BULK FORCE, volume force

A force distributed over the volume of a material. It is characterized by a volume force density f , i.e. a force acting upon a unit body volume. An example is a mass force f that acts on mass and is associated with the acceleration a of a body: f = −ρa, where the density ρ can depend on the position, and vary throughout the body. The force of gravity f G (at the Earth’s surface f G = ρg, where g is the acceleration of gravity) is a special case of a mass force. Other volume forces are: a thermoelastic force (see Elasticity theory, Thermoelasticity); the forces of electric and magnetic ﬁelds acting upon charges and magnetic moments, respectively; and the force acting upon the body from the conduction electrons that drift in an electric ﬁeld E, f = enE (here n is the number of conduction electrons per unit volume, e is the electron charge). BULK MODULUS, compressibility modulus One of the elastic moduli of an isotropic medium, K; it is expressed via the Lamé coef cients

as K = λ + (2/3)μ. Its reciprocal value is called the compressibility. In crystals of cubic symmetry, K = (c11 + 2c12 )/3 (here cik are the secondorder elastic moduli in Voigt notation). The bulk modulus is measured in pascals. K is 0.77 GPa for Al; 1.37 for Cu; 1.78 for Fe; 0.75 for Ge; 0.24 for NaCl; 4.00 for diamond. BULK PHOTOVOLTAIC EFFECT

The appearance of a stationary photocurrent under uniform illumination of a macroscopically homogeneous piezoelectric (see Piezoelectricity) or ferroelectric crystal. A bulk photovoltaic effect was discovered in the late 1960s which exhibited a linear dependence of the photocurrent on the light intensity (see Glass’ constant). The effect leads to the generation of photoelectric voltages which can exceed the band gap width by several orders of magnitude, and are limited only by the photoconductivity of the crystal. The direction and magnitude of the photocurrent depend on the orientation of the light polarization. Linear and circular effects are known. Phenomenologically, it is convenient to establish the characteristics of the bulk photovoltaic effect by expanding the photocurrent Ii in a power series of the electric ﬁeld Ej as Ii = σij Ej + αij k Ej Ek∗ + γij i EE ∗ j + · · ·

142

BULK SOUND HARDENING

The ﬁrst term with the second-rank tensor σij describes photoconductivity in an external ﬁeld Ej . The second term describes the linear bulk photovoltaic effect (i.e. in linearly polarized light); Ej and Ek being the projections of the light polarization vector. The components of the third-rank tensor αij k of this effect differ from zero for only 20 piezoelectric symmetry groups. The third term describes the circular photovoltaic effect. The microscopic theory of the bulk photovoltaic effect takes into account two basic mechanisms. The ﬁrst, so-called ballistic, mechanism is related to the asymmetry of the distribution function of the nonequilibrium carriers in momentum space. This asymmetry, in its turn, is caused by the asymmetry of the generation, recombination, and scattering of the nonequilibrium carriers in a crystal without a center of symmetry. The second, so-called shift mechanism, is due to displacement of the center of gravity of the wave packet of an electron during its optical transition between bands, or between an impurity center and a band in a crystal without a center of symmetry. The two mechanisms describe both intrinsic and impurity bulk photovoltaic effects, and predict similar magnitudes of the bulk photovoltaic effect. Therefore, the experimental differentiation of these mechanisms is a complicated task. At present, the linear and circular effects are observable in a large number of ferro- and piezoelectric crystals, including ferroelectric niobates and tantalates, Te, GaAs, GaP, ZnS, and some other piezosemiconductors.

can control processes of homogenization, recovery, recrystallization, and phase transitions. A speciﬁc feature of the action of intensive vibrations on a material is the nucleation and growth of microcracks (see Crack) at early stages of loading, a fatigue type phenomenon. Depending on the conditions of treatment, and the initial state of materials, acoustic dehardening may occur, e.g., with sound waves incident on initially deformed metals with a face-centered cubic lattice. BURGERS CONTOUR

A contour constructed in a regular crystal lattice by sequentially tracing a closed line from one atom to another. It is used to classify defects in crystals, and is of particular importance for the description of linear defects or dislocations (Fig. (a)). If a dislocation appears in a crystal enclosed with such a contour, the contour remains open. In order to close a Burgers contour, it must be complemented with a vector called a Burgers vector that closes the break (Fig. (b)). A Burgers vector b characterizes a dislocation unambiguously. Linear needle-shaped defects of different types unconnected with translational slip of a part of a crystal

BULK SOUND HARDENING, sonic strengthening An increase of the yield limit, microhardness

and other mechanical properties, observable during propagation of high-intensity elastic waves (sonic waves) in solids, mainly in metals. For every material in equilibrium there is a critical vibration amplitude, which depends on the ambient temperature and frequency. It is starting from this amplitude that the density of dislocations, vacancies and other defects of the crystal structure increases. The shape and the size of a mechanical part remains practically unchanged in this case, which is an advantage of this method of hardening (see Strain hardening). Bulk sound hardening can arise due to the intensiﬁcation of thermally activated processes. Using the latter, one

Burgers contour in a defect-free crystal (a) and in a crystal with an edge dislocation (b). In the latter case, the Burgers contour is closed with the Burgers vector b.

BURSTEIN–MOSS EFFECT

relative to another part (chain of vacancies, chain of impurity atoms, etc.) never cause a break of a Burgers contour. Sometimes a closed Burgers contour is constructed within a crystal with a dislocation (Burgers contour in the Frank interpretation). Then, upon removal of the dislocation from the crystal, the Burgers contour turns out to be open, and it is closed by a Burgers vector. When dealing with small-angle and large-angle grain boundaries, use is also made of a special Burgers vector constructed in the reference lattice (contour in Frank’s interpretation). This contour is constructed with the help of similar (according to the crystallographic direction) vectors drawn in neighboring grains so that the vectors originate from the same point located at the boundary. The Burgers contour is closed in this case with the closure vector B. BURGERS EQUATION (J.M. Burgers, 1940)

An equation of the form Ut + U Ux − μUxx = 0, where U (x, t) is the velocity ﬁeld; x, t are space and time coordinates, subscripts indicate partial differentiation, and μ is the viscosity coefﬁcient. The equation is a one-dimensional reduction of the Navier–Stokes equations (see Continuum mechanics), and is the simplest member from among the most important equations of the physics of nonlinear waves. Burgers equation gives a good description of the dynamics of weakly nonlinear waves in continua, including solids, when only ﬁrst order dissipation effects are taken into account. The complete solution of Burgers equation is connected with the Cole–Hopf transformation (J.D. Cole, 1951; E. Hopf, 1950): U = −2μ(ln ϕ)x , which transforms the former into the linear diffusion equation: ϕt − μϕxx = 0. If there is no dissipation (μ = 0), then the nonlinearity causes a gradual increase of the wave front slope, and ﬁnally leads to the formation of a break (simple Riemann wave). The latter, increasing in the presence of viscosity (μ > 0), leads to the intensiﬁcation of dissipation effects that seek to decrease the proﬁle slope. It is the mutual compensation of these contradicting trends, represented in Burgers equation by the last two terms, that brings about the possibility of the propagation of waves with a stationary proﬁle, including a shock wave with a ﬁnite shock width, directly propor-

143

Closed dislocation line in a crystal: A is the region unaffected by the shift; B is the region where a shear deformation has occurred; Burgers vector b is indicated.

tional to μ and inversely proportional to the shock amplitude. BURGERS VECTOR (J.M. Burgers, 1939)

The most important translational characteristic of linear defects in crystals is the Burgers vector (b) which closes an open Burgers contour around a dislocation line. When there is no dislocation, the contour is closed. The magnitude and direction of a Burgers vector determine how a portion of material on one side of the dislocation line is shifted relative to the material on the other side (see Fig.). A Burgers vector and a tangent vector of the dislocation line determine the slip plane of a dislocation element. In magnitude, a Burgers vector can equal either a whole repetition period of the crystal lattice in the vector direction (for perfect dislocations) or equal a fractional part of it (for partial dislocations). A Burgers vector is constant along the entire length of a dislocation line, whatever its conﬁguration, and remains constant during the dislocation motion. The sum of Burgers vectors of dislocations meeting at a dislocation site equals zero if all the dislocation lines are directed either to or from the site (Frank networks). Elastic strains and stresses produced by a dislocation in a crystal are proportional to the magnitude of the Burgers vector, while the strain energy is proportional to its magnitude squared. When dealing with smallangle and wide-angle grain boundaries in crystals, a closure vector B is introduced, which is similar to a Burgers vector and is caused by the presence of dislocations at the boundary. This vector carries the information on the angle of disorientation of neighboring grains. BURSTEIN–MOSS EFFECT (E. Burstein, T.S. Moss, 1954) An upward shift in energy of the intrinsic light absorption edge in semiconductors accompanying

144

BURSTING

an increase of the free current carrier concentration. The Burstein–Moss effect is due to ﬁlling the bottom of the conduction band by electrons in n-type semiconductors or the top of the valence band by holes in p-type semiconductors. Then, only states above the Fermi level E F are available for transitions involving photoexcited carriers. As a result, direct optical band-to-band transitions at T = 0 K are possible with the energy of quanta satisfying the inequality 2 kF2 mn 1 + , ω ωmin = Eg + 2mn mp

where E g is the band gap, mn and mp are the effective masses of the electron and the hole, respectively; and k F is the wave vector corresponding to the Fermi level. At T > 0 K and mn /mp 1, the magnitude of the Burstein–Moss effect is approximately equal to Δω = E F −4k B T in directgap semiconductors, and in semiconductors with small mn (e.g., InSb), it already appears at carrier concentrations 1017 cm−3 . The Burstein–Moss effect is used in studies of the energy band structure of semiconductors. BURSTING See Penetration deformation.

Cc in cadmium polycrystal at T melting is 1.7·10−12 m2 /s. Effective high-energy (3 to 10 MeV) neutron cross-section for absorption and scattering is 4.3 barn, and 2610 barn for thermal (0.025 eV) neutrons. Ion-plasma frequency is 8.54 THz; lowtemperature linear electronic speciﬁc heat (Sommerfeld coefﬁcient) is 0.70 mJ·mole−1 ·K2 ; electrical resistivity is 83.6 n·m (at 293 K) along the principal axis 6 of a monocrystal and 68.7 n·m in a perpendicular direction at room temperature, thermal coefﬁcient of electrical resistance in these directions is 0.0041 and 0.00405 K−1 , respectively; Hall constant is ∼ = + 5.7·10−11 m3 /C at room temperature. Work function of cadmium polycrystal is 4.1 eV. Critical temperature of cadmium transition to the superconducting state is 0.517 K; critical magnetic ﬁeld is 2.8 mT (at 0 K). Cadmium is a diamagnetic material with molar magnetic susceptibility −19.7 · 10−6 CGS units (at 300 K); nuclear magnetic moment of 111 Cd isotope is −0.592 nuclear magnetons. Cadmium is used in nuclear power engineering and as a component of alloys for solders, printing blocks, jewelry, electrodes.

CADMIUM, Cd

Chemical element of Group II of the periodic system with atomic number 48 and atomic mass 112.41. Natural cadmium consists of stable isotopes with mass numbers: 106 (1.215%), 108 (0.875%), 110 (12.39%), 111 (12.75%), 112 (24.07%), 113 (12.26%), 114 (28.86%), 116 (7.58%). The electronic conﬁguration of the outer shells is 4d 10 5s 2 . Successive ionization energies are 8.994, 16.908 eV. Atomic radius is 0.148 nm; radius of Cd2+ ion is 0.097 nm. Oxidation state is +2. Electronegativity is ∼ =1.5. In free form, cadmium is a silvery-white forgeable and ductile metal. It has a hexagonal closepacked crystal lattice; a = 0.297912 nm, c = 0.561827 nm (at 298 K). Density is 8.65 g/cm3 at 293 K; T melting = 594 K; T boiling = 1030 K. Bond energy is 1.16 eV/atom at 0 K. Heat of melting is 6.38 kJ/mole; heat of sublimation is 112.2 kJ/mole; heat of evaporation is 99.9 kJ/mole; speciﬁc heat is 0.231 kJ·kg−1 ·K−1 ; Debye temperature is ∼ =200 K; coefﬁcient of the linear thermal expansion of cadmium monocrystal is 54.0·10−6 K−1 along the principal axis 6 and +19.6·10−6 K−1 perpendicular to it (at 300 K); coefﬁcient of thermal conductivity is 83.7 W·m−1 ·K−1 along the principal axis 6 and 105 W·m−1 ·K−1 perpendicular to it (at room temperature). Adiabatic coefﬁcients of elastic rigidity of cadmium monocrystal: c11 = 114.5, c12 = 39.5, c13 = 39.9, c33 = 50.85, c44 = 19.85 (in GPa) at 300 K; bulk modulus is ∼ =58 GPa; Young’s modulus is ∼ =65 GPa; shear modulus is ∼ =25 GPa; Poisson ratio is ∼ =0.31 (at 300 K), ultimate tensile strength is ∼ =0.08 GPa and relative elongation is ∼ =32%. Brinell hardness is ∼ =0.18 GPa. Cadmium is easily forged and rolled. Surface tension of liquid cadmium is 0.628 J/m2 (at 623 K). Self-diffusion coefﬁcient of atoms

CADMIUM SULFIDE

A semiconductor compound of the AII BVI group (see Semiconductor materials), which crystallizes in the cubic sphalerite structure (zinc ¯ blend structure), space group F 43m (Td2 ), and in the hexagonal wurtzite structure, space group 4 ). The unit cell of sphalerite P 63 mc (C6v contains four molecules with lattice parameter a = 0.5835 nm, while that of wurtzite contains two molecules, with lattice parameters a = 0.41368 nm, c = 0.6713 nm, and the ratio of anion and cation radii is 0.52. For both structures the tetrahedral positions of the atoms is characteristic, the crystals have no center of symmetry, 145

146

CALAMITICS

they are polar; they form polytypes (see Polytypism) as derivatives of basic structures. Below the pressure 3 GPa a transition to the structure of sodium chloride is observed. The cubic modiﬁcation is stable at considerably lower temperatures than those of growing monocrystals. Data given for the hexagonal wurtzite modiﬁcation are as follows: temperature coefﬁcients of linear expansion with temperature reduction from 600 to 150 K are reduced from 5.9·10−6 to 0.5·10−6 K−1 , density is 4.825 g/cm3 , melting temperature is 1748 K, heat of formation ◦ = −157 kJ·mole−1 , standard entropy

Hf,298.15

◦ = 71 J·mole−1 ·K−1 , speciﬁc heat S298.15 ◦ Cp,298.15 = 47.4 J ·mole−1 ·K−1 , heat conduc-

tivity 0.20 W·cm−1 ·K−1 , Debye temperature is 219.3 K. Covalent bonding prevails with some admixture of ionic bonding. The phonon spectrum has nine optical and three acoustic branches. The band gaps are direct, the valence band presents three closely located subbands: Γ9 (the upper one), Γ8 , Γ7 ; the ﬁnal conduction band has symmetry Γ7 . The band gap width: Eg,1.8 K = 2.58 eV, Eg,300 K = 2.53 eV. Average values of temperature coefﬁcient of Eg variation at constant pressure (dEg /dT )P in the range 90 to 300 K and coefﬁcient (dEg /dP ): −5.2·10−4 eV/K and 3.3·10−6 eV/bar. The spin– orbit interaction constant is 0.065 eV, the valence band splitting due to the crystal e ld action is 0.027 eV, electron af nity is 4.73 eV, work function is 7.26 eV. Effective masses of electrons, holes: m∗n = 0.205, m∗p = 0.7 (⊥ c), m∗p = 5 ( c). Refraction index dispersion and birefringence are characterized by the values: ne = 2.726, no = 2.743 at λ = 515 nm; ne = 2.312, no = 2.996 at λ = 1500 nm. Static and high-frequency dielectric constants are: εs = 8.64 ( c), εs = 8.28 (⊥ c), ε∞ = 5.24. The Cd–S system in the phase equilibrium diagram has one compound CdS with a narrow range of homogeneity. Inherent atomic defects to a large extent determine the diffusion and solubility of impurities, the structure of local centers, optical and electric properties. Elements of Group III Al, Ga, In, can replace the cations, elements of Group VII Cl, Br, I, replace the anions, vacancies of anions, interstitial cations are shallow hydrogen-like

donors; elements of Group I Cu, Ag, replace the cations, cation vacancies behave as deep acceptors. The association of the point defects is characteristic. Conductivity may change from a semimetal to insulator type, no p-type conductivity is observed due to the self-compensation phenomenon. Mobility of electrons and holes: 350 cm2 ·W−1 ·s−1 and 30 cm2 ·W−1 ·s−1 . Minority carrier lifetimes (holes) are 10−6 to 10−8 s, diffusion lengths of holes are short (7 to 0.5 μm). The presence of direct band gaps facilitates effective luminescent and laser radiation. Blue radiation is caused by the annihilation of free and associated excitons, green, orange, red and infrared radiations are associated with impurity recombiA = nation. At T 15 K energy of excitons Eex B C 2.550 eV, Eex = 2.564 eV, Eex = 2.632 eV, bonding energies of excitons: EA = EC = 0.0294 eV, EB = 0.0295 eV. Centers of radiative recombination are centers of photosensitivity. Having the high photosensitivity in a wide spectral range: from UV to near IR, in the X-ray spectral range CdS is characterized by high sluggishness, low temperature and time stability of photocurrent. The absence of a center of inversion and a strong electron–phonon interaction determine the piezoelectric properties. The capability of fabrication by simple methods in the form of powders, tablets, and caked layers of thin lms with controllable properties is a pronounced advantage. The uniqueness and variety of its physical properties allows its use as a model material of the physics of semiconductors and quantum electronics: in photo-, opto-, acoustoelectronics, optics, laser engineering. Cadmium sulphide is widely used as a crystallophor for the creation of the screens of electron tubes, including color television, as a photoconductor for the creation of photoresistors, of nuclear particles radiation sensors, as an element of heterojunctions for solar phototransformers.

CALAMITICS

Uniaxial liquid crystals with structure units (molecules or micelles) of oblong cylindrical shape (cf. Discotics).

CALORIMETRIC COEFFICIENTS

CALCIUM, Ca

Chemical element of Group II of the periodic system with atomic number 20 and atomic mass 40.078, it belongs to alkaline-earth metals. Natural calcium is a mixture of 6 stable isotopes with mass numbers 40, 42–44, 46, 48; among them, 40 Ca (96.94%) is the commonest and 46 Ca (0.003%) is the rarest. Electronic conﬁguration of outer shell is 4s 2 . Atomic radius is 0.197 nm. Successive ionization energies are 6.133, 11.872, 50.914 eV. It is chemically active; oxidation state +2. Electronegativity is 1.04. In free form, calcium is a silvery-white metal; it darkens in the air due to formation of products of calcium interaction with oxygen, nitrogen, water vapors, etc., at the surface. From room temperature to 716 K, α-Ca is stable with face-centered cubic lattice (with parameter a = 0.556 nm); at temperatures above 716 K and up to T melting = 1120 K β-Ca is stable with a body-centered cubic lattice (with parameter a = 0.448 nm), T boiling = 1770 K. Density of α-Ca is 1.55 g/cm3 . Heat of melting is 8.4 kJ/mole; heat of evaporation is 152 kJ/mole; speciﬁc heat cp = 25.9 J·mole−1 ·K−1 . Work function 2.75 eV. Debye temperature is 220 K; temperature coefﬁcient of linear expansion is 2.2·10−5 K−1 (at 273 to 573 K); heat conductivity is 125 W·m−1 ·K−1 ; electrical resistivity is 3.8·10−2 μ·m (at 273 to 373 K); temperature coefﬁcient of electrical resistance is 4.57·10−3 K−1 . Hall constant is −1.78·10−10 m3 /C; magnetic susceptibility is χ = +1·10−9 . Modulus of normal rigidity is 21 to 28 GPa, tensile strength is 59 GPa, elastic limit is 4 MPa, limiting yield stress is 37 MPa. Brinell hardness is ∼250 MPa. Metallic calcium is used in metallurgy for reduction of U, Th, Zr and other rare metals from their compounds; as deoxidizing and degassing agent in melting of special steels, bronze, etc. Calcium is used as a getter in electronic devices. Monocrystals of the calcium compound, ﬂuorite CaF2 , ﬁnd wide use in optical and laser devices. CALIFORNIUM, Cf

Chemical element of Group III of the periodic system with atomic number 98 and atomic mass 251.08, belongs to actinides. There are no stable isotopes, and 17 radioactive isotopes are known

147

with mass numbers 240 to 256. Electronic conﬁguration of outer shells of atom is 5f 9 6d 1 7s 2 . Atomic radius is 0.169 nm; ionic radius of Cf3+ is 0.906 nm. Oxidation state is +3 (less often, +2, +4, +5, +6). Electronegativity is 1.23. In free form, californium is a silvery metal. It exists in two allotropic modiﬁcations: lowtemperature (α-Cf) and high-temperature (β-Cf). The ﬁrst has a hexagonal close-packed crystal 4 ), a = 0.3988 nm, (space group P 63 /mmc (D6h c = 0.6887 nm at room temperature); according to other data, it has a double hexagonal close-packed crystal lattice (a = 0.339 nm, c = 1.101 nm). The other modiﬁcation has a face-centered cubic lattice (space group F m3m (Oh5 ), a = 0.5743 nm and a = 0.494 nm upon hardening by quenching at ∼1000 K and 870 K, respectively) at temperatures above 860 K to T melting = 1170 K. T boiling ≈ 1500 K. Density of α-Cf is 15.1 g/cm3 . Below the Curie point T C = 51 K, α-Cf transforms from a paramagnetic state to a ferromagnetic one; in β-Cf, no magnetic ordering has been found. Californium isotopes (in particular, 252 Cf) are used as neutron sources in activation analysis, in medicine, etc. Californium is highly toxic. CALORIMETRIC COEFFICIENTS

The thermodynamic coefﬁcients of the form (∂Q/∂μ)ν where μ and ν take on the values of any of the thermodynamic parameters P , V , T (pressure, volume, temperature) of a system. The quantity ∂Q is the amount of heat transferring the system into a new thermodynamic state under a variation of μ by ∂μ at ν = const. There are 6 principal calorimetric coefﬁcients: (∂Q/∂T )V = CV , speci c heat at constant volume, (∂Q/∂T )P = CP , speciﬁc heat at constant pressure, (∂Q/∂P )T , heat of isothermal compression, (∂Q/∂P )V , heat of isochoric compression, (∂Q/∂V )P , heat of isobaric expansion, (∂Q/∂V )T , heat of isothermal expansion. The calorimetric coefﬁcients can be expressed via the derivatives of the thermodynamic state functions: enthalpy H and internal energy U (see

148

CALORIMETRY

Thermodynamic potentials):

∂Q ∂T V ∂Q ∂T P ∂Q ∂P T ∂Q ∂P V ∂Q ∂V P ∂Q ∂V T

∂U , ∂T V ∂H = , ∂T P ∂H = − V, ∂P T ∂U = , ∂P V ∂U = + P, ∂V P ∂U = + P. ∂V T =

In addition to calorimetric coefﬁcients, thermodynamics also makes use of six thermal coefﬁcients: (∂V /∂P )T , (∂P /∂T )V , (∂T /∂V )P , (∂V /∂P )S , (∂P /∂T )S and (∂T /∂V )S , where S is the entropy. There are 9 independent thermodynamic relationships between these 12 thermodynamic coefﬁcients so only 3 thermodynamic coefﬁcients can be selected as independent ones to be evaluated theoretically or determined experimentally. In principle all other coefﬁcients can be calculated via these three, chosen as independent. This circumstance allows one to calculate coefﬁcients that are difﬁcult to measure experimentally through easily measurable ones. For instance, ∂P ∂V 2 , CV = CP + T ∂V T ∂T P ∂V ∂P ∂T = −1, ∂P T ∂T V ∂V P ∂P ∂P ∂H =T +V . ∂V T ∂T V ∂V T

Instruments for calorimetric measurements are called calorimeters. Their design is determined by the temperature interval and desired accuracy. The two most widely used types in studies of solids are adiabatic calorimeters where the heat exchange between calorimeter and medium is negligibly small, and dynamic (heat-conducting) calorimeters based upon detection and control of the heat ﬂux between the sample and the environment. Adiabatic calorimeters with a pulse heat input are very accurate for measurements made close to equilibrium. They are used at temperatures from 0.05 to 1000 K to determine the speci c heat, thermodynamic functions, latent heats of phase transitions, the critical index α of phase transitions; density of states of electrons at the Fermi level N(EF ) by the electronic speciﬁc heat coefﬁcient γ ; obtaining direct information on energy levels of valence electrons by the Schottky effect; investigation of energy properties of vacancies and coordination polyhedra. A drawback of this method is the long time required for making the measurement. Dynamical calorimeters, in particular the Calve type, are used at temperatures from 77 to 1880 K. The temperature variation rate is from 1 K/h to 64 K/min. The important advantage of calorimeters of this type is the possibility of contact between the sample and the environment, control of the pressure or gas phase during the experiment, and access to the center of the calorimeter when necessary. The ﬁeld of application is the determination of heat capacities, thermodynamic functions, latent heats of phase transitions, heats of oxidation–reduction reactions, heats of gas–solid reactions, the energy related to the strain of a solid, and heats of adsorption and desorption. At temperatures above 1800 K the speciﬁc heat of solids is determined by the offset method. Benzoic acid and corundum have been adopted as standard substances in calorimetry.

CALORIMETRY (fr. Lat. calor , heat, and Gr. μετρεω , am measuring)

CANONICAL TRANSFORMATION METHOD (N.N. Bogolyubov, 1947)

Methods for measuring thermal effects accompanying different processes. Calorimetric methods are used in the interval 0.05–3500 K and attain an accuracy 0.01%. Calorimetry at temperatures above 400 K is conventionally called a hightemperature type.

A method utilizing a unitary transformation of particle creation ak+ and annihilation ak operators in order to reduce the initial complex Hamiltonian of a many-particle quantum system, involving interacting particles expressed in a second quantization representation, to a simpler Hamiltonian in

CAPACITANCE

diagonal form for noninteracting quasi-particles with a restructured energy spectrum. If the initial Hamiltonian has the form 1 1 ∗ , H= Ak ak+ ak + Bk ak a−k + Bk∗ ak∗ a−k 2 2 (1) then by introducing new operators according to the relations + , ak = λk ck + μ∗k c−k

+ + a−k = λ∗k c−k + μk ck (2) the Hamiltonian assumes the form H = ε(k)ck+ ck + E0 , (3) 1/2 ε(k) = A2k ∓ |Bk |2 .

The parameters of the canonical transformation obey the normalization condition |λk |2 ∓ |μk |2 = 1. In formulae for the energy of the quasi-particles and the transformation parameters the upper sign corresponds to bosons and the lower sign corresponds to fermions. The canonical transformation for spin waves was applied by Holstein and Primakoff (1940) to a ferromagnetic material, and it was applied by Bogolyubov (1947) to bosons for the case when many of them are in the state of a Bose–Einstein condensate (see Bose–Einstein condensation). The method was exploited by Bogolyubov to construct his microscopic theory of superconductivity (1947). It results in the following elementary excitations: 2 2 2 k 2 2 , (4a) E(k) = k u (k) + 2m NV (k) u(k) = , (4b) m where m is the boson mass, N is the number of particles in a unit volume, and V (k) is the Fourier transform of the pairwise interaction potential. For particles with repulsion, when V (k) > 0, Eq. (2) yields at k → 0 the acoustic dispersion law of quasi-particles E(k) ≈ ku(0), which is a necessary but insufﬁcient condition for the super uidity of neutral Bose systems (see Landau super uidity criterion). When attraction dominates at large distances with V (0) < 0, the spectrum (2) at k → 0

149

becomes unstable (imaginary), which corresponds to an exponential growth of long-wavelength perturbations in time, and a spontaneous contraction (collapse) of the system. For charged bosons (e.g., bipolarons) with a long-range Coulomb repulsion V (k) = 4πe2 /k 2 (e is the boson charge), the spectrum (2) of quasi-particles at k = 0 has a ﬁnite energy gap E(0) = ωp (ωp is the plasma frequency) and satisﬁes the superﬂuidity criterion, which corresponds to superconductivity (see Bipolaron mechanism of superconductivity). In the case of electrons (fermions) interacting under the conditions of Cooper pairing (see Bardeen–Cooper–Schrieffer theory) one can use Hamiltonian (1), where k denotes both the momentum and the spin of the electron, and Ak and Bk are given by Ak = ξ(k),

Bk = Δ(k).

Here ξ(k) is the energy measured from the Fermi level, and Δ(k) is the non-zero energy gap below the transition temperature from the normal to the superconducting (superﬂuid) state of a Fermi system. In the self-consistent eld approximation, which is asymptotically accurate in the thermodynmic limit (see Bogolyubov method in the theory of superconductivity), transformations (2) lead to a reconstructed spectrum of quasiparticles in a superconductor with the energy ε(k) = [ξ 2 (k) + Δ2 (k)]1/2 . CAPACITANCE

A quantitative measure of the ability of an object or material to retain electric charge q. Charged particles of the same sign attempt to go out of a charged body due to electrostatic repulsion. Mobile charge carriers in a conducting medium spread over its surface and provide an equal value of electric potential ϕ everywhere on the surface. If the conductor is electrically charged then its potential differs from that at inﬁnity where by convention ϕ∞ = 0. The value ϕ is proportional to q; and it speciﬁes the conductor capacitance by the ratio C = q/ϕ. The greater the value of C, the greater the charge on the conductor at a given ϕ. The magnitude C of an isolated conductor is determined by its geometric dimensions and shape; e.g., the capacitance of a sphere is equal to its

150

CAPACITANCE, BARRIER

radius (in Gaussian system of units). In a system of conductors, a correspondence between their charges and potentials is determined by the linear

relations qi = j Cij ϕj (Cij is called the capacity coefﬁcient of the ith and j th conductors). In a system metal–insulator–metal (condenser), the capacitance is determined by the relation C = q/ ϕ where q is the value of charges of opposite sign on every capacitor plate; ϕ is the potential difference between the plates. For a planar capacitor C = εA/d where A is the area of each plate, d is the distance between them, and ε is the relative (dimensionless) dielectric constant of the medium between the plates. For a very small d, the capacity of the system can be very large. The systems metal–semiconductor, semiconductor junction, and so on are similar to a capacitor, and can also have a signiﬁcant capacitance (see Barrier capacitance). Variations of the thickness of the dielectric layer under actions of any kind provide information on the distribution of electrically active extended defects in a system (see Capacitance–voltage characteristic, Capacitance spectroscopy). Josephson junctions, with typical capacitances C ∼ 10−15 F, exhibit voltage changes V = e/C ∼ 0.016 mV for individual electron tunneling. This is called a Coulomb blocade, and it appears on a current versus voltage characteristic curve (I versus V , or dI versus dV plot) as a sequence of steps called a Coulomb staircase. CAPACITANCE, BARRIER See Barrier capacitance. CAPACITANCE SPECTROSCOPY

A collection of methods for determining the energy spectrum of deep levels in semiconductors from changes in their barrier capacitance, C, during variation of the applied voltage. A simple version of capacitance spectroscopy is based on measuring steady-state capacitance–voltage characteristics. When a reverse bias (i.e. a bias in the cut-off direction) is applied to a system containing a semiconductor junction or a Schottky barrier, the thickness L of the semiconductor region with depleted current carriers increases, and the capacitance of the depletion layer decreases. More information can be obtained by methods of nonstatic capacitance spectroscopy of deep levels. It

is based on the measurement of the capacitance relaxation kinetics for different combinations of factors applied to ﬁll or ionize the deep levels (such as forward and reverse bias pulses of various durations, photoionizations, and temperatures). Using these methods provides separate measurements of concentrations of deep levels with different ionization energies, and also determines the cross-sections of charge carrier trapping at the levels. The efﬁcient Lang method measures the differences between C at two times, t1 and t2 , during the course of the relaxation of C with the emission of electrons or holes from individual levels into a corresponding allowed band. There are modiﬁcations of this method when the relaxation of current rather than capacitance is measured; and taken together they constitute the relaxation spectroscopy of deep levels. CAPACITANCE, SURFACE See Surface capacitance. CAPACITANCE–VOLTAGE CHARACTERISTIC

Dependence of the sample capacitance C on the applied voltage V . Measurement of the capacitance–voltage characteristic is one of the most widespread methods of investigating semiconductor electron–hole transit, heterojunctions, Schottky diodes and metal– insulator–semiconductor structures. From the shape of a C–V characteristic it is possible to determine the distribution of doping impurity in the structure. In particular, in sharp p–n junctions and Schottky diodes the capacitance–voltage characteristic plotted as C −2 versus V is a straight line with a slope characterizing the doping of the semiconductor, and the cutoff voltage is equal to the equilibrium height of the potential barrier at the junction (contact potential difference). The characteristic shape of the C–V characteristic for M–I–S structures is shown in the ﬁgure. The presence of deep levels within the bulk or at the surface of the sample, which recharge during voltage variations, causes additional features of the capacitance–voltage characteristic. Besides, the shape of the C–V characteristic has a strong dependence on the frequency f of the probing signal, because at high frequencies there is not enough time to recharge the deep levels, and to

CARBIDE TRANSFORMATIONS

Dependence of the capacitance on the voltage in an M–I–S structure at a low (solid line) and a high (dashed line) frequency, where C0 is the insulator capacitance.

form the inversion layer in the M–I–S structure. This allows one to use the C–V characteristic and its frequency dependence to obtain information about the concentration, energy spectrum and trapping proﬁles of the bulk and surface levels (see also Varicap, Capacitance spectroscopy). CAPILLARY PHENOMENA

Physical phenomena arising from surface tension. Capillary phenomena are most easily observed in thin tubes (R 10−3 m). The fundamentals of capillarity theory laid by P.S. Laplace (1806–1807) include two basic laws: (1) the excess pressure under the curved surface of liquid is 1 1 , (1) +

p = ±σ R1 R2 where σ is the surface tension coefﬁcient, R1 and R2 are the radii of curvature of two mutually perpendicular sections of the surface at the point in question; and (2) the edge angle θ0 of a solid surface by a liquid is independent of the shape of the surface. Of importance in the theory is the capillary constant a with the dimensions of length: σ , (2) a=

ρg where ρ is the difference between the densities of the phases in contact, and g = 9.8 m/s2 . For cylindrical tubes the Borelli–Jurin equation holds 2σ cos θ0 h= , (3) gRρ where h is the height of the rise of the wetting liquid and ρ is the liquid density. Eq. (3) describes the impregnation of pore structures, and

151

substantiates the role of capillary forces in the root feeding of plants utilized for soil tillage. Eq. (1) explains the presence of a considerable capillary counter-pressure in a system of alternating drops of liquid and gas bubbles in capillaries (gas embolism, decompression sickness in divers). See also Thermocapillary effect, Electrocapillary phenomena. CARBIDES (fr. Lat. carbo, coal, and Gr. ειδoς , type) Chemical compounds of carbon with metals

and some nonmetals. We can distinguish covalent carbides (beryllium carbide, boron carbide, silicon carbide), metal-like, and salt-like carbides. Metal-like carbides include those of scandium, yttrium, lanthanum, lanthanides, transition metals of Groups IV to VII of the periodic system, and metals of the iron family. Carbides of transition metals (TiC, Cr3 C6 , Cr3 C2 , Mo2 C, WC and others) are interstitial phases and structures close to interstitial, with the carbon atoms occupying octahedral or tetrahedral sites (voids) of close-packed metal lattices. Such carbides exhibit metallic characteristics of conductity, high melting (decomposition) temperature, hardness and chemical stability. Salt-like carbides include those of s-state metals (alkali, alkaline-earth metals and aluminum). The best known among them is calcium carbide CaC2 , a colorless crystal, with density 2.21 g/cm3 , T melting ∼ 2300 ◦ C. Carbides are obtained from elementary matertials in vacuo or in a reducing gas atmosphere, as well as by interaction of metallic oxides with carbon in vacuo or in a reducing atmosphere, by interaction of metals or their oxides with carbon-containing gases, and by interaction of gaseous compounds of some metals (halides) and carbon in the hydrogen atmosphere. The favorable properties of carbides are used in nuclear and space engineering, microelectronics, metal processing and many other areas. CARBIDE TRANSFORMATIONS in steel

Formation and rearrangement of iron carbides during the course of different treatments of steel. Carbides are one of the basic phases in steel; they may form upon cooling of steel heated above some critical point, or upon tempering of hardened steel (see Quenching). Above 300 ◦ C a stable iron carbide, cementite, is present in carbon steel. At the tempering of alloyed steels, the temper-

152

CARBON

ature of cementite (Fe3 C) formation increases. Redistribution of carbon and alloying elements between phases leads to alloying of iron carbide. With a certain temperature of tempering, degree of steel alloying, and ratio of carbide-forming element content to that of carbon, the formation of special carbide is possible. Destabilization of cementite (or special carbide) occurs at complete replacement of one atom of iron in cementite (or the basic element in special carbide) with the alloying element. In multicomponent alloying such replacement occurs with several alloying elements simultaneously. Carbide transformations that run according to the mechanism of alloy aging and direct precipitation of carbides from ferrite, bypassing cementite, are used to harden structural, stamp, tool, high-speed and certain austenite steels, as well as to maintain hardening in long-term operation of boiler and turbine, motor equipment, of industrial holders and fastening parts, etc., at increased temperatures. The speciﬁcs of redistribution of carbon and alloying elements between phases in multicomponent alloying causes the carbide transformations to run at a lower number of alloying elements than in single or simple alloying (and the same total degree of alloying). Here, the ferrite contains more alloying elements, which permits a more complete use of their effect upon physical mechanical, technological and service properties of steel. The composition and type of the carbide crystal lattice, distribution of carbides within the structure, and the mechanism of their formation are investigated using chemical phase analysis, X-ray structure analysis, microscopic diffraction and magnetic analyses, Mössbauer spectroscopy, internal friction, and electron microscopy with the help of replicas and foils. CARBON, C

The chemical element of Group IV of the periodic table with atomic number 6 and atomic weight 12.011. The mass numbers of the two stable carbon isotopes are 12 (12 C, 98.892%) and 13 (13 C, 1.108%). The 14 C isotope is unstable (halflife 5730 years). The wide diversity of properties of carbon compounds is due to the electronic conﬁguration of the carbon atom: 1s 2 2s 2 2p2 . Interaction with other atoms results in rearrangement

of the density of the electron clouds and the concentration of electron density in certain directions, such as along chemical bonds (see Hybridization of orbitals). Depending on the way atomic orbitals are combined, sp-, sp2 - and sp3 -hybridizations are distinguished. Each hybridization corresponds to a particular spatial arrangement of a bond. Oxidation states of carbon in its compounds are −4, −2, +2, and +4; electronegativity value is ≈2.58; atomic radius 0.077 nm, ionic radii: 0.016 nm for C4+ and 0.26 nm for C4− . There exist ﬁve allotropic (see Allotropy) modiﬁcations of solid carbon: diamond (sp3 -hybridization of orbitals), graphite (sp2 -hybridization), fullerene (C60 and analogues, sp2 -hybridization), carbyne (sp-hybridization), and amorphous carbon (mixed type of bonding). Carbyne is a quasione-dimensional semiconductor, the width of the band gap of which is ∼1 eV. Amorphous carbon is a polyphase structure, which consists of the ﬁnest inclusions of polymorphic modiﬁcations of carbon. Depending on the mode of preparation, carbon may also contain chemically bound hydrogen atoms, which saturate the dangling bonds of the carbon structure. The principal carbon-containing minerals are salts (carbonates) of carbonic acid H2 CO3 . Carbon atoms are the chief constituents of coal, oil, peat and other materials. Carbon is a nonmetal and behaves as an active reducing agent on heating. It forms carbides with various elements, e.g., boron carbide, silicon carbide SiC, cementite Fe3 C. Carbon is used as a reducing agent, as a component of various alloys, as fuel, for production of electrodes, etc. CARBON, ACTIVE See Active carbons. CARBON FILM, DIAMOND-LIKE See Diamond-like carbon lms. CARBYNE (fr. Lat. carbon , coal)

The third allotropic modiﬁcation of carbon, which consists of rectilinear carbon chains bound into crystals through van der Waals forces. The rectilinear shape of the chains is due to sp-hybrid bonding of the carbon atoms. In actual samples the individual chains are cross-linked, with perhaps some periodicity, and this involves a transition of

CASTING MATERIALS

some carbon atoms into sp2 - or sp3 -hybrid type bonding. The presence of carbyne can be detected by the methods of electron diffraction and X-ray diffraction. Crystalline particles of carbyne are colorless, and no large monocrystals have been prepared. Carbyne is hard to obtain in a pure form (free from admixture of laminated modiﬁcations of carbon). Density and other physical properties depend on the method of manufacture and puriﬁcation. Carbyne has a higher speci c heat than graphite and diamond, and it surpasses graphite in hardness. Heat of combustion is 84 to 372 kJ/mole, which is signiﬁcantly lower than that of graphite and diamond, which attests to the thermodynamic stability of carbyne. There are 3 bands in the Raman spectrum of carbyne at 1360, 1580 and 2140 cm−1 , the last of them being the characteristic one related to the vibrations of conjugate C–C bonds. Carbyne is an n-type semiconductor with a band gap of 0.64 eV; electrical resistivity is 106 ·cm (at 293 K). Carbyne was originally obtained and characterized by the methods of oxidative polycondensation of acetylene. It forms upon condensation from vaporgas phase, plasma, an ion-molecular beam under the conditions that are softer compared to those for forming diamond, and of laminated polymers of carbon. Natural carbyne was discovered in 1968 in a meteorite crater and received the name chaoite (white veins and disseminations in graphite). In its chemical inertness it surpasses graphite and approaches diamond. Defect-free thread-like crystals of carbyne are believed to have very high rupture strength. CASCADE, COLLISION See Collision cascade. CASTING

The process of forming pieces (casts) by ﬁlling a hollow casting form or mold with melted material (metals, their alloys, plastics, certain rocks, metallurgy slags). The principal advantages of casting include the possibility of obtaining casts of a complicated conﬁguration that is as close in size and shape to the ﬁnal product as possible. Mold casting of steel, cast iron, nonferrous alloys (from 5–10 to 100 g and more in mass) is used

153

to produce various parts, from time-piece components to heavy-duty constructions for engineering, metallurgy, power and other branches of machine building. Steels and alloys are cast into molds (plate casts, forging casts) or poured continuously into water-cooled crystallizers (for a continuously operating casting installation). More than 50 types of casting techniques are available. Traditional technologies include pouring molten metal from dippers or crucibles driven by gravity into sand casting forms. Special casting techniques make it possible to improve the quality of casts, perform precision casting in both size and shape, and achieve special physical and mechanical characteristics. Such technologies involve various external factors which act upon the crystallizing metal and provide for using special casting forms, models or casting techniques. Among the latter are casting under high or low pressure, centrifugal casting, electric slag casting, continuous or suspension casting, casting into melted-out models, casting into chill molds, ceramic and shell forms, etc. Art casting is done using melted-out models to produce monumental sculptures, architectural decorations, and jewelry. CASTING MATERIALS

Macroscopically inhomogeneous substances obtained by fusion of two and more mutually soluble metals, nonmetals, or organic substances, and by subsequent solidi ca tion of the liquid phase in a mold of a particular shape. Depending on the temperature range of metastability of the liquid phase, the structure of casting materials may be crystalline or amorphous. In a general case, the conditions of solidiﬁcation in the amorphous or crystalline states may be controlled by the cooling rate, by the purity of the materials, by their solubility, and by their crystallization activity. The properties of casting materials crystallizing during the course of solidiﬁcation are not only determined by their chemical composition, by the method of fusion, thermal and other types of deformationless treatment, but are also dependent on the thermal conditions of solidiﬁcation, on the nucleation rates of centers, and the linear growth rates of crystallization nuclei. These factors determine the degree of development of physical, chemical and structural inhomogeneities in

154

CAST IRON

casting materials. The processes of their solidiﬁcation and crystallization, and hence their properties, may be signiﬁcantly changed by modi cation, electromagnetic mixing and other methods (see Casting). CAST IRON

Alloy of iron with carbon (usually 2 to 4% C), also containing (Si, P and S, Mn), and sometimes additional alloying elements (Al, V, Cr, Ni, etc.); it solidiﬁes with the formation of eutectics. Unlike steel due to its low plasticity, cast iron is machinable under pressure. It is characterized by a high liquid yield. Cast irons are subdivided into the following classes: pearlite, ferrite, perlite-ferrite, sorbite, troostite, bainite, martensite, troostite-ferrite, and austenite. According to its microstructure the following types are distinguished: gray cast iron (in the form of cementite or iron carbide Fe3 C), and forgeable cast iron obtained by annealing white cast iron (ﬂocculent graphite). The properties of cast iron are improved by alloying, modi cation, thermal treatment. Cast iron is the primary product obtained from the processing of iron ore materials. It is used in chemical, petroleum, and agricultural machine building, in tool, car and tractor fabrication, in civil engineering, etc. CATALYSIS, RADIATION See Radiation catalysis. CATASTROPHE, POLARIZATION See Polarization catastrophe. CATEGORY (fr. Gr. κατ ηγ oρια , accusation)

A level of crystallographic classiﬁcation by the number and order of special (or individual) directions, i.e. directions in the crystal lattice which do not repeat under a symmetry operation (see Crystal symmetry). There are three categories: the highest one (no special direction and some symmetry axes of order higher than 2); the medium type (one special direction along a unique symmetry axis of order 3, 4, or 6); the lowest one (no special direction and no symmetry axes of order higher than 2). The highest category involves crystals of the cubic system, the medium one includes those of the hexagonal system, trigonal system and tetragonal system, and the lowest category encompasses structures of the orthorhombic system,

monoclinic system and triclinic system. Depending on the category the nature of the anisotropy, and many physical properties of a solid change characteristically (see Anisotropy of crystals). This classiﬁcation term “category” is not commonly used in the Western literature. CATHODE See Cold cathode, Field-emission cathode, Thermionic cathode, Photocathode. CATHODE SPUTTERING See Sputtering. CATHODOLUMINESCENCE A type of radioluminescence excited by an

electron beam (“cathode rays”). Depending on the electron energy E, one distinguishes low-voltage (E = 10–100 eV) and high-voltage (E > 0.5 keV) cathodoluminescence. At high-voltage the electrons overcome the surface barrier, penetrate to a depth proportional to E 1.4 , knock out secondary electrons that also ionize atoms, create electron– hole pairs, or directly excite the ions of the activator (Mn2+ , Tb3+ and others). The minority carriers migrate across the lattice and are trapped at luminescent centers, accompanied by radiative recombination. At low voltage the excitation by primary electrons only covers several near-surface atomic layers, and the diffusion of nonequilibrium carriers produces a zone of ﬂuorescence spreading into the depth of the sample. The forming negative charge is neutralized at high voltage luminescence mainly through the emission of electrons from the surface of a luminophor, while at low voltage the neutralization is due to the conductivity of the latter. In its spectrum, cathodoluminescence is similar to other types of luminescence. Its brightness in a certain spectral region is proportional to E and the current density in the beam. The energy yield is 10–30% for high voltage and 0.5–2% for low voltage. Cathodoluminescence is employed in picture tube screens and in low-voltage indicators that are used in devices for the visualization of information, TV sets and other electronic devices. Cathodoluminescence underlies the operation of lasers excited by an electron beam.

CATLOW–DILLER–NORGETT POTENTIAL

155

CATLOW–DILLER–NORGETT POTENTIAL (C.R. Catlow, K.M. Diller, M.J. Norgett, 1977)

A central pair-potential that describes shortrange ion-to-ion interactions in ionic crystals using the shell model. An analysis of the relation between the equilibrium interionic distance in a crystal and its elastic constants on the one hand, and the interionic interaction potentials yielded by this model for alkali-halide crystals (such as LiCl, NaCl, KCl, RbCl) on the other hand, demonstrated that the ion-to-ion interaction is attractive at long distances r and repulsive at short distances. Starting with that observation, Catlow, Diller and Norgett offered the following two proposals for the short-range potential of (identical) second nearest neighbors in alkali halides. I. The Buckingham potential V (r) = A exp(−r/ρ) − Cr −6 contains an exponential repulsive term with parameters A, ρ determined using an electron gas model, and an attractive van der Waals potential with a parameter C (see Van der Waals forces). For example, the F− –F− ionic interaction in a LiF crystal is described by A = 1128 eV, ρ = 0.02753 nm, and C = 12.71 eV·nm5 . The parameters for the anion–anion (C−− ) and cation–cation (C++ ) interactions are arbitrarily assumed to be equal to each other, C−− = C++ = C/2. II. A combined (“spline”) potential consists of expressions used in proposal I for attraction at long distances and repulsion at short ones, plus the third and ﬁfth power polynomials for intermediate distances (see Fig.): V (r) = −Cr −6 , V (r) =

3

r > ra ,

(1)

ai r i ,

ra > r > rm ,

(2)

bi r i ,

rm > r > rb ,

(3)

i=0

V (r) =

5 i=0

r , V (r) = A exp − ρ

rb > r.

(4)

Matching the functions at points ra , rb , and at the minimum point rm is carried out by invoking continuity of the functions and their

Schematic represention of the potential described in proposal II for the four regions: (1) r > ra , (2) ra > r > rm , (3) rm > r > rb , and (4) rb > r.

ﬁrst derivatives. The parameters A and ρ coincide, while C considerably exceeds the value expected from proposal I. For example, C = 26.8 eV, while ra = 0.3457 nm, rb = 0.2 nm, rm = 0.2833 nm for the F− –F− interaction. These parameters are self-consistently adjusted over the entire alkali halide series. Having ﬁxed the potential parameters for second nearest neighbors, one may update the respective parameters for ﬁrst neighbors, that is for adjacent ions, that potential being the common Born– Mayer potential, V (r) = A exp(−r/ρ). Next the parameters of the ions are determined using the shell model. The shell charge and the nucleus– shell bonding constant are found by comparing the static and the high frequency dielectric constants and the transverse optical frequencies with experimental data for all the crystals, so that the polarization of a crystal may be adequately described by the result. The Catlow–Diller–Norgett potential, as presented in II above, has a number of advantages over other potentials used for ionic crystals. It covers every individual ion and is easily applied to modeling alkali halides. It offers a consistent picture of the ion-to-ion interaction for all the alkali halides. In combination with the Coulomb potential it adequately describes the properties not only of an ideal crystal, but of a real one as well. In the

156

CAUCHY RELATIONS

latter the ion-to-ion distances may differ considerably from the equilibrium ones in the vicinity of defects. Thus it becomes possible to study both intrinsic crystalline and impurity defects in various ionic crystals (see Interatomic interaction potentials). CAUCHY RELATIONS (A. Cauchy)

Additional relations between the 36 crystal elastic moduli cik following from the symme-

tries of interatomic interactions, where i, k = 1, 2, . . . , 6. If the interatomic forces are pairwise and central then each term is at a center of symmetry, the undeformed crystal is stress free, and the harmonic approximation is valid. Then in the general case there are 21 independent modulus constants cik (in Voigt notation) by virtue of the symmetry condition cik = cki . The six Cauchy relations c12 = c66 , c13 = c55 , c23 = c44 , c14 = c56 , c25 = c46 , and c36 = c45 reduce the number of independent elastic moduli to 15. For cubic crystals there are three independent elastic constants (c11 , c12 , c44 ), and one Cauchy relation (c12 = c44 ). These results hold well for some alkali-halide crystals, but not for most other cubic crystals. In metallic crystals the Cauchy relations usually do not hold (e.g., in noble metals c12 /c44 ∼ 2–4). In elastically isotropic crystals obeying the Cauchy relations c11 = 3c44 , and the Poisson ratio is ν = 1/4. For orthorhombic crystals there are 9 independent constants and 3 Cauchy relations, corresponding to 6 independent moduli when the Cauchy relations hold. CAVITATION RESISTANCE

The ability of a material to resist the effect of cavitation (formation of vapor bubbles) that appears in a liquid at the passage of a powerful sonic or ultrasonic wave (acoustic cavitation), and also during high-speed ﬂow past bodies (hydrodynamic cavitation). The collapse of a cavitation bubble at the compression phase produces a local hydraulic shock which affects the surface of a tool, an article, or a part. Cavitation erosion is especially strong for brittle materials such as rocks, concrete, and ceramics. Metals possess considerably higher cavitation resistance that reduces noticeably in hostile media and suspensions with abrasive particles, and upon increasing the pressure within the

volume of a liquid. Ultrasound is widely applied in some technological processes where cavitation plays an important role, and this has prompted the search for materials with high cavitation resistance. Its measure is the loss of mass per unit area during a preset period of time. The cavitation intensity is evaluated by the destruction of a thin aluminum foil placed in the cavitation area. There are also other methods to determine cavitation resistance in investigations of hydrodynamic cavitation, such as rotational, jet-impact, and ﬂowthrough ones. CAYLEY TREE (A. Cayley, 1889); also called a Bethe lattice

A branched structure in which each site has f nearest neighbors, and no two branches are permitted to cross each other. It is cycle-free, and also self similar since each branch is itself an entire tree. Such graphs are used for percolation studies, in cluster techniques to provide a convenient boundary condition for a cluster, to calculate the number of isomers of saturated hydrocarbons, and to describe disordered solids. CELLULAR STRUCTURE

Regions 1 μm in size which are free of dislocations, or which contain individual dislocations, dislocation dipoles, multipoles, interlacements, networks, etc., and are separated by dislocation interlacements, balls, or rods. The cell boundaries can be either dense or spread out, either narrow or wide, and so on. The cells can be equiaxial or nonequiaxial. Sometimes the cellular structure is called block-cellular structure (see Block structure). CEMENTATION

Coating a metal, usually iron or steel, by heating it with another substance so that the added material, usually a powder, diffuses into the surface; it is a type of chemical heat treatment. The coating material might be a metal like aluminum or zinc, or perhaps carbon. Diffusion saturation of a steel product surface by carbon typically produces a saturated layer that is 0.5 to 2 mm thick, with a carbon content of 0.8–1.1%. Cementation with subsequent quenching and low annealing provides articles with a high surface hardness, wear resistance and increased fatigue strength, leaving their

CENTRAL FORCES

core tough. Cementation may be carried out in gaseous, liquid, and solid media containing carbon. It is used in the production of tools. CEMENTITE (fr. Lat. caementum , broken stone) A structural component of steel and cast iron containing the elements iron and carbon. Cemen-

tite is the most stable iron carbide (Fe3 C), containing 6.7 wt.% C (see Carbide transformations). It is formed upon the cooling of iron–carbon alloys (see Iron alloys) if the conditions are favorable for crystallization to occur in the metastable phase diagram of these alloys (iron–cementite). Cementite is often a component of pearlite, sorbite, troostite and ledeburite. The crystal lattice of cementite is orthorhombic; the unit cell contains 12 atoms of Fe and 4 atoms of C. Lattice constants are: a = 0.4514 nm, b = 0.5079 nm, c = 0.6730 nm. According to some indications cementite is close to an interstitial phase (see Interstitial alloys). It forms substitutional solid solutions: carbon may be replaced by nitrogen or oxygen, iron by manganese, chromium or tungsten (alloyed cementite). Their dispersity, the form of cementite crystals, and their crystal structure associated with a ferrite environment (see Ferrites), to a large extent determine the strength and plasticity of iron–carbon alloys after a heat treatment. Cementite is hard and brittle, and there is practically no elongation if it fails during the course of tensile tests. The melting temperature is ∼1873 K; at this high temperature it decomposes into austenite and graphite. It is ferromagnetic with the Curie point of 486 K. CENTER See Active centers, Amphoteric center, Color center, Dilatation center, Luminescent centers, Paramagnetic center, Positron center, Positronium center. CENTER OF INVERSION See Center of symmetry. CENTER OF MASS, center of inertia

A point in a solid body relative to which the total ﬁrst moment of the all the components of the mass vanish, i.e. i mi r i = 0, where r i is the radius-vector of the ith mass relative to the center of mass. In the absence of torques a solid body

157

moves as if the resultant sum of all applied forces R = i F i were acting at the center

of mass, and the total mass of the body M = i mi were concentrated there. This deﬁnition implies that the center of mass is, in a uniform gravitational ﬁeld, the center of gravity, as well as the point where the resultant force of gravity Mg is acting. CENTER OF PERCUSSION

The point of a body about which it starts to rotate when an impulse (impulsive force) is applied at another point in the body. CENTER OF SYMMETRY, center of inversion

A special point of a ﬁgure possessing the property that during the inversion operation (r → −r) through that point as origin of coordinates, all the elements (points) of the ﬁgure transform into themselves (r is the coordinate of an arbitrary point of the ﬁgure). The presence of a center of symmetry is equivalent to the presence of an inversion axis of the ﬁrst order. Many properties of the solid state depend on the presence or absence of a center of symmetry; see, e.g., Electric e ld effects in radio-frequency spectroscopy. CENTI. . . (fr. Lat. centum , a hundred)

Preﬁx to the name of a physical value to form a fractional unit equal to 1/100 of the source unit. Abbreviation symbol is c. For instance, 1 cm (centimeter) = 0.01 m. CENTRAL FORCES

In solids these are forces of interaction between pairs of atoms (ions) acting along the straight line connecting them. In such a case these atoms are considered to be point masses. Formally the concept “central forces” is based on “rigid” point atoms (ions). When interatomic interactions in solids are described exclusively by means of central forces, this constitutes a coarse and phenomenological approximation. The central force is a special case of a pairwise interaction between atoms, when its adiabatic potential U has the form 1 U= ϕ |R i − R j | , 2 ij

where R i is the radius-vector of the lth atom, and ϕ is a function which depends on the type of interaction. For a gravitational ﬁeld involving two

158

CENTRAL PEAK

masses ϕ = −Gm1 m2 /|R 1 − R 2 |, corresponding to an inverse square central force law, where G is the gravitational constant.

dering point. This central peak is due to the contribution of nonlinear spin excitations, i.e. magnetic solitons.

CENTRAL PEAK

CERAMIC FERROELECTRIC See Ferroelectric ceramics.

A sharp increase of the magnitude of the order parameter u ctuation at a frequency approaching zero in the neighborhood of the critical point Tc of a structural phase transition. Initially a central peak was observed in 1971 in the energy spectrum of a beam of monochromatic neutrons scattered by a SrTiO2 crystal in the vicinity of Tc = 105 K. Central peaks have also been observed experimentally in spectra of Raman scattering of light. Depending on the nature and mechanism of its formation one should distinguish three types of central peaks: static intrinsic, static dynamic, and impurity types. A static intrinsic central peak is associated with the relaxation of lattice distortions of crystals without impurities. The mechanisms of dynamic intrinsic central peak formation are much more diverse. These involve ﬂuctuations of the entropy (ferroelectrics: SrTiO2 , KTaO3 , KDP type), the presence of an overdamped soft mode at T → Tc (K2 SeO4 ), two-phonon anharmonic interactions (germanate of Pb, SrTiO2 ), diffusion of mobile ions in solid electrolytes (Ag, F, β-alumina), formation of a paraphase, and relaxation at T → Tc of clusters of the prior ordered phase. The impurity central peak is associated with the relaxation of defects which differ from the point of view of a given central peak formation by the symmetry of their local surroundings, and by the rigidity of their coupling with a crystal lattice. Direct experiments on KPD-type crystals have shown that the central peak disappears at the annealing of defects. In the phenomenological theory the integrated intensity of a dynamic intrinsic central peak at T → Tc increases as the susceptibility (at a given external ﬁeld), and its width is 1 to 2 orders less than an impurity central peak width. For example, in NaNO3 the central peak width is ∼1013 s−1 , which is an order of magnitude less than the central peak width in KH2 PO4 . A central peak was found when quasi-one-dimensional magnetic materials (ferromagnetic CrNiF3 , antiferromagnetic KMnF3 , etc.) were examined at temperatures higher than the three-dimensional or-

CERAMIC GLASS See Glass ceramics. CERAMIC PIEZOELECTRIC See Piezoelectric ceramics. CERAMICS (fr. Gr. κεραμικoς , made of clay)

A baked (sintered) material; pottery. A class of compact materials, based on the compounds that the nonmetallic elements of Groups III and IV of the periodic system form with one another and/or with metals, produced by technological processes that allow for mass transport, as well as for the binding of the components. Classiﬁed as ceramic materials are: glass (see Vitreous state of matter), monocrystals of refractory materials, and composites with a ceramic matrix (see Composite materials). Traditional (Table 1) and novel ceramics may be distinguished. The vast majority of ceramic materials are mono- or heterophase polycrystalline materials based on high-melting compounds. A wide diversity and intricacy of the electronic structure of high-melting compounds comprising different types of interatomic bonds (covalent, ionic, metallic) results in a unique combination of properties (high energy of fragmentization, hardness, refractory properties, large elastic moduli, a collection of distinctive electrophysical properties, etc.). Their spatial distribution of interatomic bonds is related Table 1. Types of traditional ceramics • Pieces of Art • Household pottery and china (tableware and tiling, crockery, bathroom particulars, etc.) • Glass (a variety of items and materials for all areas of application) • Binding materials (cement, gypsum, lime, mortar, etc.) • Construction materials (pipes, bricks, roof tiles, etc.) • Fire prooﬁng materials (bricks, crucibles, etc.) • Abrasive materials

CERAMICS

159

Fig. 1. Typical scheme of the production technology of ceramics.

to diamond-like crystals with predominantly covalent bonds (carbides, silicon nitride and boron nitride), and these substances all have similar structures constructed on the principle of diversiﬁed sequential packing of identical layers. These compounds are characterized by the existence of a substantial number of polytypes (see Polytypism); the latter have also been found in diamond. Besides covalent and ionic crystals, there are many ceramic material components from a large group of metal-like high-melting compounds, such as interstitial solutions that form easily in transition metals by light elements with relatively small atomic radii. Most of these phases are compounds of variable proportion having wide ranges of homogeneity, and a great variety of structure types (e.g., CaFe, ZnS, CaB6 , etc.). Conventionally the properties of a ceramic are deﬁned not only by the properties of its

components, but to a substantial degree, by the technology of production (Fig. 1). Also widely employed are the methods of self-propagating high-temperature synthesis, chemical sedimentation, inﬁltration from the gas phase, etc. The stability of the crystal lattice and the low mobility of defects in high-melting compounds results in low rates of the diffusive and viscous processes responsible for mass transport, and for settling at the solid-phase sintering. For that reason, additives to activate the sintering are introduced into the batch charge, and this is then subjected to explosion processing to augment the number of defects, or there could be a physical and chemical modi cation of the surface, etc. The activating additives, usually oxides, secure the liquid-phase sintering regime, which not only facilitates the rearrangement of component particles, but also results in their recrystallization via the liquid phase. This ac-

160

CERAMICS Table 2. Properties of several types of alumina Type of ceramic

Fig. 2. Microstructure of ceramics fabricated by way of the processes: (1) solid-phase sintering, (2) liquid-phase sintering with the formation of (A) solid solutions, and (B) systems comprising a crystalline matrix with glassy phases at grain boundaries; (3) crystallization of eutectic liquids; obtaining composites of crystalline matrix with thread-like crystals (4), or with ﬁbers (5), by solid- or liquid-phase sintering, or by the chemical sedimentation and inﬁltration from the gas phase.

Strength, GPa

Type of defects

An ideal crystal, theoretical strength

50

–

Whisker thread-like crystals

15

Screw dislocations along the axis of growth, and surface defects

Single crystals

7

Surface and bulk defects of crystal lattice

Hot-pressed ceramic

0.8–1.0 Same as above, plus grain boundaries and additional phases

Sintered technical ceramic

0.2–0.3 Same as above, plus pores

celerates the sintering process, while permitting a substantial decrease in the temperature, but the ceramic thus fabricated will be interlayered with an amorphous phase at grain boundaries. Typical microstructures obtained with such processes are presented in Fig. 2. The type of microstructure that is realized, as well as the character of the defects and inhomogeneities in the ceramic, determine its mechanical behavior and its complex of physicochemical properties resulting, for instance, in a variation in strength by over two orders of magnitude (see Table 2). The wide variety of types of structure, and sometimes the attainment of record values of the physical properties of the phase components of the ceramics, provides us with the opportunity for fabricating unique materials for a large number of purposes. Along with the attainment of high strength (more than 1500 MPa), a high fracture toughness can be achieved to compensate for the traditional brittleness. The “viscous” state is not only reached by means of a “skeletal” reinforcement, but also because the processes of elastic energy dissipation are being purposely initiated at the vertex of a spreading crack; the effects of such processes are similar to the action of plastic relaxation at crack vertices in metals. In ceramics, the energy dissipation is conditioned by the development of microcracks, by ﬁrst- and second-order phase transitions, etc. The stability to cracking of such

CERIUM Table 3. Fields of application of novel (reﬁned, advanced) ceramics • In electrical engineering and circuit electronics (substrates, varistors, magnetic, ferroelectric and hightemperature superconducting ceramics, transducers, sensors, etc.) • Structural ceramics (engine parts in the aerospace and automobile industries, facing materials, fairings, thermoresistive bearings, heat exchangers, special ﬁreproof materials, etc.) • In medicine (implants, bio-ceramics, etc.) • In nuclear technology (nuclear fuel, materials for nuclear reactors, etc.) • Wear resistant ceramics • Low weight armor • Fiber and laser optics, etc.

a ceramic may be enhanced from a typical level of K 1c = 1–3 MPa·m1/2 up to values in the range of 10–30 MPa·m1/2 , viz., up to a magnitude characteristic of hard alloys and some metallic construction materials. The discovery in 1986 of high-temperature superconductivity in copper oxides, and the raising of the critical temperature of superconductors up to 90–135 K for ceramics of the type of YBa2 Cu3 O7−δ (123 phase) and HgBa2 Ca2 Cu3 O8+δ , respectively, opened up essentially new opportunities in superconductor electronics. All the superconducting cuprate ceramics are type II superconductors, possess a perovskite-like structure (see Perovskites), and have a carrier current density smaller than that of metals and alloys, the carriers generally being holes (in some cases electrons). The 123 phase, the ﬁrst one discovered with T c above 77 K, has granular particles of 1–10 μm dimensions that are in weak electrical contact with each other in the ceramic body, with the electromagnetic properties of the ceramic strongly inﬂuenced by intercrystallite grain-boundary layers. On the whole, there is a broad range of applications of these novel ceramics (Table 3), and these materials are used in many ﬁelds of technology. CERIUM, Ce

Chemical element of Group III of the periodic system with atomic number 58 and atomic mass 140.12; it is the lightest rare-earth element

161

aside from lanthanum. Natural cerium has 4 stable isotopes 136 Ce (0.193%), 138 Ce (0.25%), 140 Ce (88.48%) and 142 Ce (11.07%). The outer shell electronic conﬁguration is 4f 2 5d 0 6s 2 . Ionization energies are 6.9, 12.3, 19.5, 36.7 eV. Atomic radius is 0.181 nm; radius of Ce3+ ion is 0.107 nm, of Ce4+ ion is 0.094 nm. Oxidation states are +3, +4. Electronegativity is 1.08. Cerium is a silvery-blue metal; in air it is covered by a grayish-white oxide ﬁlm. Four crystalline modiﬁcations of cerium are known (α-Ce, β-Ce, γ -Ce, δ-Ce). The crystal lattice of α-Ce is face-centered cubic with a = 0.485 nm (at 77 K); β-Ce has a double hexagonal close-packed lattice (α-lanthanum type), a = 0.3673, c = 1.1802 nm (at 298 K); γ -Ce is face centered cubic with a = 0.51612 nm (at 293 K); δ-Ce has a body centered cubic lattice, a = 0.411 nm (at 1041 K). At room temperature γ -Ce is stable. During the course of cooling, starting from the temperature 263 K, γ -Ce partially transforms to β-Ce; the transformation is of a martensitic nature. At the temperature ∼95 K the non-transformed part of γ -Ce transforms to α-Ce. Below 77 K β-Ce also transforms to α-Ce, but this transition is not completed even at the temperature of liquid helium 4.35 K. The complete transition may be achieved only by plastic deformation of the sample at 77 K. The transitions γ ↔ α and γ ↔ β are characterized by large hysteresis depending on the temperature and pressure. At atmospheric pressure the reverse transformations α → γ and β → γ start from the respective temperatures ∼160 K and ∼373 K. If the pressure is over 2500 atm β-Ce cannot exist at any temperature. The behavior of Ce strongly depends on its history and purity. The transformation γ ↔ δ takes place at 998 K. Density is 6.678 g/cm3 at 293 K, Tmelting = 1071 K, Tboiling = 3740 K. Heat of melting is 9.211 kJ/mole, heat of evaporation is 390.18 kJ/mole, heat of sublimation is 398 kJ/mole; speciﬁc heat is 27.9 J·mole−1 ·K−1 at 298 K; coefﬁcient of thermal conductivity is 10.89 W·m−1 ·K−1 at 300 K, linear expansion coefﬁcient is 8.5·10−6 K−1 at 298 K. Electrical resistivity is 0.753 μ·m at 298 K, temperature coefﬁcient of electrical resistance is 8.7·10−4 at 273 K. Above 12.5 K cerium is paramagnetic with molar magnetic susceptibility +2300·10−6 .

162

CERMET

Thermal neutron cross-section is 0.63 barn. Debye temperature is 139 K. At room temperature the elastic modulus is 29.99 GPa, shear modulus is 11.99 GPa, Poisson ratio is 0.248; ultimate tensile strength of cast sample is 0.1206 GPa, relative elongation is 32.6%. Pure cerium is a forgeable and tough metal. At room temperature without preheating it is possible to manufacture cerium sheets by forging, and wire by pressing. It is used as an alloying addition to the light metals, and also as a getter. CERMET (fr. ceramic metal)

A composite material consisting of ceramic grains dispersed in a metallic matrix. It is formed by techniques of powder metallurgy. CESIUM, Cs

Chemical element of Group I of the periodic table with atomic number 55 and atomic mass 132.9054. There is one stable isotope 133 Cs, and 22 radioactive isotopes, among which 137 Cs with a half-life 27 years has found the broadest applications. Outer shell electronic conﬁguration is 6s 1 . Ionization energies are 3.893, 25.1, 34.6 eV. Atomic radius is 0.262; radius of Cs+ ion is 0.167 nm. Oxidation state is +1. Electronegativity is 0.68. Cesium is a silvery-white metal. It has a bodycentered cubic lattice with a = 0.605 nm (at 448 K). Density is 1.9039 g/cm3 (at 273 K) and 1.880 g/cm3 (at 300 K); Tmelting = 301.75 K; Tboiling ≈ 960 K. Heat of melting is 15.8172 kJ/kg, heat of evaporation is 613.2 kJ/kg; speciﬁc heat at constant pressure is 32.2 J·mole−1 ·K−1 at 298 K; thermal conductivity ratio is 16.7 to 27.2 W·m−1 ·K−1 at 301.6 K; linear expansion coefﬁcient is 9.7·10−5 K−1 (273 to 300 K). Electrical resistivity is 0.183 μ·m (at 273 K) and 0.2125 μ·m (at 300 K). Mohs hardness is 0.2; Brinell hardness is 0.015. Normal elastic modulus is 1.716 GPa at room temperature. Debye temperature is 42 K. Ion-plasma frequency is 1.724 THz; linear low-temperature electronic speciﬁc heat coefﬁcient is ≈3.20 mJ·mole−1 ·K−2 . Electronic work function of cesium polycrystal is ≈1.85 eV. Cross-section of thermal neutron trapping is 29 barn. Cesium is paramagnetic with magnetic susceptibility 0.1·10−6 (at 291 K).

Cesium is used in the production of photocells (it exceeds all the other metals in light sensitivity), of gas absorbers, and of low work function coatings for emitters. The application of “cesium plasma” is prospective for ionic reactor motors. CHAIN REACTIONS

Reactions of active particles (free radicals in chemical reactions, neutrons n in nuclear reactions), when the elementary interaction produces one or a number of additional active particles (radicals, A·). In the ﬁrst case the reaction is called an ordinary, non-branched chain reaction, in the second case it is a branched one. The chlorination process of H2 : Cl· + H2 → HCl + H·, Cl2 + H· → HCl + Cl·, . . . , etc., is an example of a non-branched chain reactions. The process of H2 oxidation represents an example of a branched chain reaction: H· + O2 → ·OH + O:, O: + H2 → ·OH + H·, ·OH + H2 → H2 O + H·, . . . , etc. In such a manner, the primary species A· may give rise to a large number (from ten to 107 ) of transformations of inactive particles (e.g., molecules). The number of such transformations per primary active species A· is called the chain length. The breaking of a chain (chain reaction termination) may be due to the presence of an impurity which interacts with A· so an additional A· is not produced. Also it may be due to the departure of A· from the reaction region. In the simplest situation (homogeneous case) the chain reaction rate is determined by the equation: v = K1 C1 P0 t × exp

(α − 1)K1 C1 − K2 C2 dt − βt ,

0

where P0 is the concentration of the primary species A· created by the initiating chain reaction, K1 and K2 are the velocity constants of chain reactions and the chain breaking reaction; C1 and C2 are the concentrations of initial substances of the chain reactions, and of the chain breaking centers; α is the number of A· species arising in the elementary act of chain initiation; β is a constant related to the probability of A· leaving the reaction region. The exponential term in this equation reﬂects the time change of the radical concentra-

CHALCOGENIDE MATERIALS

tion; and the relations between the terms in the exponent index determine the kinetic character of the chain reactions. So, if the ﬁrst term in the exponent index turns out to be larger than the sum of the others, then the chain reactions velocity increases exponentially with respect to time, and a chain explosion is possible. In solids chain reactions have been found in organic matrices. The matrix itself and also the components diluted in it can participate in these reactions. For example, in organic polymeric matrices which contain halide complexes of Au, Pt, Cu, Bi chain reactions can be initiated by the action of light or ionizing radiation on the system. As a result, atomic Cl· appears (e.g., [AuCl4 ]− +Cl· → [AuCl2 ]− +Cl2 +Cl·), and the chain length in such systems may reach 104 . The use of chain reactions for the photographic recording of information provides new opportunities for the creation of sensitive media with high resolution. Free radicals giving rise to chain reactions may be generated at the heterogeneous burning of solids and its mixtures in the reaction zone. In such a case the very existence these radicals determines the burning kinetics. There is some evidence that at burning, chain reactions also occur in the condensed phase. Nuclear chain reactions take place in uniform solid specimens of U-235 or Pu-239 (nuclear bomb), and also in the case of a nonuniform distribution of U-235 in some other material (graphite, heavy or light water, or of course U-239) which form the nuclear reactor. The ﬁrst nuclear chain reaction was realized by E. Fermi in 1942 in a uranium-graphite reactor. Up to the present time only uranium nuclear reactors are in use, and they satisfy the following conditions. The elementary act of ﬁssion involves a neutron n striking a U-235 nucleus in accordance with the reaction U-235 + n → A + B + kn + Q, where A and B are nuclear fragments (daughter nuclei), k is the neutron multiplication factor, and the chain reaction proceeds because the average value of k ∼ 2.5 for the elementary act of ﬁssion. The kn secondary neutrons in turn induce further ﬁssions The energy Q of the reaction is harnessed

163

in nuclear power plants for heating cities, producing electricity, etc. and the number of neutrons generated is greater than one (i.e. k > 1). The cross-section of the ﬁssion reaction of U-235 increases with the decrease of the neutron velocity v as 1/v, and there are resonances in the range of neutron energy from a fraction of an electronvolt to perhaps a hundred electronvolts. As a result, the so-called “thermal neutrons” play the main role in ﬁssion reactions. At these low energies the crosssection for the U-235 ﬁssion reaction is much larger than the cross-sections for other reactions with neutrons. Since there is a large probability that many neutrons will escape from a very small sample without reacting, there is a critical mass for the chain reaction to take place, and this is approximately 50 kg for U-235 and 10 kg for Pu-239. If the average neutron multiplication factor k is too large, the number of neutrons in the specimen can grow exponentially, leading to an explosion. To prevent this, neutron absorbing rods (e.g., graphite) are inserted into the reactor to remove excess neutrons and keep k ∼ 1 so the chain reaction will proceed slowly, and generate heat gradually. CHALCOGENIDE MATERIALS (fr. Gr. χαλκoς , copper and γ ενναω, engender)

Compounds of elements of Group VI of the periodic table (O, S, Se, Te, Po, collectively called chalcogens) with other elements. The class of chalcogenides (oxides, sulﬁdes, selenides, tellurides) contains the X−2 anion of Group VI elements. In view of their differences in properties and ﬁelds of application, oxides are often unfairly excluded from the list of chalcogenide materials, and polonium compounds are rarely included because they are strongly radioactive. In modern areas of engineering chalcogenide materials are often used in the form of thin lms or monocrystals, which are obtained through precipitation of aqueous solutions, decomposition of chelate compounds on a substrate, crystallization from gaseous (vapor) phase, etc. Typical ionic lattices of chalcogenides are characteristic of these elements, which exhibit very low values of ionization potentials. Many chalcogenide materials form lattices of the chalcopyrite type, the spinel type, and others. They are often nonstoichiometric compounds. Chalcogenides comprise a broad class of

164

CHANNELED PARTICLE FRICTION

compounds, including insulators, semiconductors and conductors of electric current. Chalcogenide materials are used in opto- and microelectronics, power engineering, in metallurgy, as photosensitive elements, transparent contacts, contactless switches, image converters, light indicators and electric phosphors, resistive salts, memory storage cells, etc. Historically the term chalcogenide was used for ores and minerals containing copper and sulfur: chalcopyrite (copper pyrite) CuFeS2 , the most important of all copper ores; chalcocite Cu2 S; chalcanthite CuSO4 ·5H2 O (blue vitriol), chalcostibite CuSbS2 , and others. CHANNELED PARTICLE FRICTION See Friction of channeled particles. CHANNELED PARTICLE SELF-ACCELERATION

A phenomenon observed during the passage of a beam of relativistic charged particles through a monocrystal in parallel to crystallographic planes or axes. Charged particles travelling in the channeling mode may radiate short-wave photons. By this action the channeling charged particles may absorb quanta emitted by other charged particles of the beam, and thereby increase their initial energy. Quasi-bound motion of charged particles in the planar or axial channneling mode may be regarded as one-dimensional or two-dimensional atoms. Thus in analogy with an atomic system, the process of self-acceleration of channeled particles may be called a quasi-Auger effect. For ultrarelativistic electrons entering a monocrystal parallel to crystallographic planes, the main radiation mechanism is electromagnetic quasi-characteristic radiation associated with the transitions of electrons from the free state to the channeling one. An electron in the quasi-bound channeling state may transfer to another quasi-bound state or escape into the continuum spectrum as a result of electron trapping (this exchange takes into account the possible contributions of not only real, but also virtual photons). The kinematics of this process shows that in the ﬁnal state it is possible to detect charged particles with double their initial energy.

CHANNELING in monocrystals

The transversely restricted (relative to the initial direction) motion of charged particles along open channels between neighboring close-packed atomic rows or planes in crystals. The condition for channeling is a small value of the angle subtended by the particle direction while entering the channel to the corresponding axis (for axial channeling) or plane (for planar channeling). This means that the particle being channeled experiences repeated glancing impacts with atoms of restraining chains (planes). These bend the trajectory in such a way that encounters with a small impact parameter become rare. The classical description of channeled ions proposed by J. Lindhard is based on using a potential averaged over the atoms of chains (planes), which is referred to as a string potential, or a continuous potential. In this case the angle ψ of the particle velocity vector relative to the axis of a chain or plane must be smaller than a critical value ψk = (U0 /E)1/2 , where E is the particle energy, and U0 is the height of the potential barrier created by the atoms of a chain or a plane. If ψ is greater than ψk , called the Lindhard angle, the particles are no longer conﬁned to the regime of channeling (see also Dechanneling). The manner of reﬂection of a particle from the walls of a channel suggests that a positively charged channeling particle spends most of its time moving past regions of a crystal with relatively low electron density. Therefore, the trapping of a particle into the channeling mode causes a reduction of its ionization energy loss and increases its effective mean free path in a monocrystal. In the channeling regime there is a considerable reduction of the probability of processes with small impact parameters relative to the sites of a crystal lattice (see Orientation effects). The occurrence of channeling was observed ﬁrst for positively charged ions, and later for electrons and positrons. It is of interest that the channeling phenomenon was “discovered” twice. In 1912, the German physicist J. Stark took notice of the fact that charged particles can penetrate to considerably greater depths along some preferential axes. However, this effect was forgotten for a long time until a “second discovery” in the early 1960s. It was found by computer

CHARACTERISTIC ENERGY LOSS

simulation that incident bombarding ions which have abnormally long paths through a monocrystal when they enter the crystal almost parallel to a main crystallographic direction. The channeling of relativistic charged particles gives rise to an intense electromagnetic quasi-characteristic radiation in the gamma ray and X-ray bands. See also Hyperchanneling, Molecule channeling, Neutral particle channeling, Quantum states of channeled particles, Okorokov effect, Channeled particle self-acceleration, Surface channeling, Surface conductive channel, Current lamentation. CHANNELING OF ION BEAMS

This takes place along the directions of atomic chains and planes in a monocrystal because the ions scattered at small angles to these directions cannot penetrate deep into the crystal (see Fig. 1). Shadow traces of the atomic chains and planes appear (the so-called shadow effect) at the target detecting the scattered ions. The emission of products of a nuclear reaction between the incident ions and the crystal atoms also produces the shadow effect. The shadow disappears, if the time

Fig. 1.

Fig. 2.

165

between the trapping of the ion nucleus by the crystal atom nucleus and the emission of the reaction product is long enough for the activated atom to displace noticeably from the blocking chain (plane). This allows one to estimate experimentally the nuclear reaction time. One can observe the blocking by the shadow effect resulting from the embedding of a radioactive isotope into a monocrystal. Fig. 2 shows the angular distribution of the intensity of emitted α-particles in a tungsten crystal upon the introduction of the 222 Rn isotope; the minimum corresponds to the 111 direction. Heating the crystal results in washing out the shadow due to thermal displacements of the atoms. CHARACTERISTIC ENERGY LOSS

Discrete energy losses, which are independent of the energy of incident primary electrons, and are characteristic of a given solid; they are observed in reﬂection and transmission spectra of secondary electrons. Characteristic energy loss is energy expended on the excitation of (i) electron transitions from inner core levels or from valence band levels to unoccupied levels, vibrational energy levels, and (ii) collective longitudinal oscillations of a solid-state plasma (plasmons). The values of characteristic energy losses of the ﬁrst kind (30–105 eV) are easily determined from the binding energies (Eb ) of electrons in atoms, and are used in ionization spectroscopy for the analysis of solids. Different solids exhibit different binding energies because of many-particle effects (relaxation, multiplet splitting, con guration interaction, shake-off and shake-up, chemical shifts). Characteristic energy losses of the second kind (1–30 eV) are more difﬁcult to interpret, since they are due to processes involving levels of the valence band and upper unoccupied levels. Vibrational characteristic energy losses are related to transitions between the vibrational states of surface atoms (molecules) of a solid, or of adsorbed layers; these characteristic energy losses are a source of information on phonon involvements. Volume and surface plasmon characteristic energy losses (ωP and ωS , respectively) are determined by the concentration of valence electrons n: ωP = (4πe2 n/m)1/2 , √ ωS = ωp / 2, and they manifest themselves

166

CHARACTERISTIC ENERGY LOSS SPECTROSCOPY

as distinct lines in the spectra of materials with weakened valence electron bonding. Other materials (e.g., transition metals) exhibit diffuse plasma characteristic energy loss lines. See also Characteristic energy loss spectroscopy. CHARACTERISTIC ENERGY LOSS SPECTROSCOPY

Branch of physics concerned with the discrete energy losses that are experienced by a monochromatic primary electron beam interacting with a solid. Characteristic energy loss spectroscopy examines samples using either the transmitted beam or the reﬂected beam of light. The techniques are applied to the investigation of inner core levels in atoms of solids, shifts of these levels caused by changes of the chemical environment, electron transitions from valence band levels to unoccupied levels, transitions among vibrational states of atoms of adsorbed layers at solid surfaces, generation of collective longitudinal plasma oscillations (plasmons). These studies provide information on the composition and electronic properties of the material as a whole, and in particular of its surface. The major ﬁelds of application are the spectroscopy of surface plasmons and vibrational characteristic energy loss spectroscopy, which allows one to perform a complete analysis of the surface. As distinct from optical spectroscopy, vibrational characteristic energy loss spectroscopy affords: (1) operation over a broad energy band (0.001–1 eV), which includes phenomena inaccessible by optical methods; (2) excitation of optically forbidden transitions, and (3) an increase of the scattering cross-section. There exists the following classiﬁcation of spectroscopic methods according to the type of physical process involved in the energy losses: ionization spectroscopy of valence and inner core levels, plasmon characteristic energy loss spectroscopy and high-resolution vibrational spectroscopy. The intensity of spectral lines due to characteristic energy losses is not very high, and decreases with an increase of the probing beam energy; therefore, electrons with energies below 2 keV are used, so the probing depth in this case does not exceed 2 nm. Thus, characteristic energy loss spectroscopy is the preferred method for examining near-surface layers of solids.

CHARACTERISTIC LENGTH OF MAGNETIC MATERIAL

Parameter lw of uniaxial magnetic materials, with the dimensionality of length, which is equal to the ratio of the surface energy density of a Bloch domain wall to the maximal volume energy density of the demagnetization eld μ0 M 2 /2. In materials with a quality or Q-factor (see Magnetic lms) exceeding 1 the characteristic length determines the minimal diameter of a magnetic bubble domain (or minimal spacing of the band domain structure), that may occur in thin layers (ﬁlms) along the easy magnetization axis, which is perpendicular to the developed surface. The largest possible diameter of an isolated magnetic bubble domain is ≈3.9lw , and the layer thickness in this case must be ≈3.3lw . CHARACTERISTIC LENGTHS IN SUPERCONDUCTORS Coherence length ξ , penetration depth of magnetic eld λ, length of imbalance relaxation λE (see Penetration depth of electric eld), Josephson

penetration depth. The superconducting phase transition is characterized by the generation of bound states, i.e. Cooper pairs of electrons which are bosons, and are subject to Bose–Einstein condensation. The coherence length ξ is the effective radius of a Cooper pair, and it determines the characteristic distances over which the complex order parameter of the superconductor ψ(r) (effective wave function of Cooper pair) changes to an appreciable extent when the superconductor is in a certain nonequilibrium state; e.g., at the penetration of Abrikosov vortices into a superconductor (ξ is the radius of the normal state vortex core), at the interface of a superconductor with a normal metal (proximity effect), etc. Typical values of ξ range from 10−6 m in pure metals to 10−9 m in alloys and compounds. The coherence length of a pure (type I) superconductor is ξ0 = vF /π 0 , and in the case of a (type II) superconducting alloy with electron mean free path ll , which is small compared with ξ0 , the coherence length at the temperature 0 K is of the order of ξ(0) ≈ (ξ0 ll )1/2 . In the neighborhood of the transition point, ξ tends to inﬁnity as ξ(T ) ≈ ξ(0)/(1 − t)1/2 , where

CHARACTERISTIC SURFACE

t = T /Tc . In a type II superconductor, the magnitude of ξ is related to the value of the upper critical e ld Bc2 through the expression Bc2 = Φ0 /(2πξ 2 ) (Φ0 = h/(2e) is the ux quantum). The Meissner effect in superconductors arises from the fact that external magnetic ﬁeld creates a current (Meissner current) in the surface layer which screens the bulk of the superconductor from the penetration of the ﬁeld. The characteristic thickness of this layer is called the penetration depth λ. In the case of a pure type I superconductor, the London penetration depth is determined from the London formula λ0 = [mc2 /(4πne2 )]1/2 and is of the order of 10−7 m. In the case of a superconducting alloy, λ > λ0 , with the value λ ≈ λ0 (ξ0 / ll )1/2 at ξ0 ll . In the neighborhood of Tc , λ has the temperature dependence λ(T ) ≈ λ(0)/(1 − t)1/2 . The penetration depth λ may be determined experimentally from the change of the superconductor inductance, which is due to partial penetration of the ﬁeld into the bulk of the solid. The imbalance relaxation length λE determines the characteristic distances of nonequilibrium processes in superconductors. The simplest case is the current ﬂow through a galvanic contact between a normal metal and a superconductor. In the normal metal, the current is carried by electrons, whereas in the superconductor it is carried by Cooper pairs. The conversion of normal excitations into pairs in the normal metal takes place at the distance λE from the interface. The electric ﬁeld E differs from zero in this region, therefore λE may be considered as the depth of penetration of a longitudinal (in contrast to the Meissner effect) “dissipative” electric ﬁeld. The nonequilibrium state of the superconductor exists within the distance ∼λE of the interface. This state is characterized by an imbalance in the occupancy of electron-like (P > PF , where PF is the Fermi momentum) and hole-like (P < PF , where P is excitation momentum) spectrum band branches. The imbalance relaxation is related to inelastic collisions (i.e. electron–phonon types), characterized by a mean free path length lε = vF τε , which are inefﬁcient at low temperatures, and therefore lead to rather high values of λE (e.g., λE ∼ 10 μm). According to theory, λE = (DτQ )1/2 , where D = vF ll /3 is the electron diffusion coef cient,

167

and τQ = [4T /(πΔ)]1/2 τε is the period of the imbalance relaxation. In the neighborhood of Tc , λE varies as λE (T ) ≈ λE (0)/(1 − t)1/4 . The value of λE determines the characteristic dimensions of the region of inhomogeneity (so-called phase slip centers) in the resistive state of superconducting ﬁlms. The Josephson penetration depth has the value λJ = [Φ0 /(2πμ0 Jc deff )]1/2 where Jc is the critical current and deff is the effective thickness of the junction. A Josephson junction is considered short when its length is less than λJ , and it is long when it has a greater length. CHARACTERISTIC SURFACE, ellipsoid

A second-order surface, which represents the orientation dependence of a particular physical property of a crystal, which is described by a second-rank tensor. The equation of the characteristic surface, when reduced to the principal axes of the crystallophysical coordinate system (e.g., an orthogonal crystal coordinate system compatible with nonorthogonal lattice constant directions) is of the form s1 x12 + s2 x22 + s3 x33 = 1, where s1 , s2 and s3 are the principal values of the tensor sij . If all sii are positive, then the characteristic surface is (in the general case) a three-axis ellipsoid; with its semiaxes equal, respectively, to (s1 )−1/2 , (s2 )−1/2 and (s3 )−1/2 , and proportional to the values of the particular physical property represented by the sij in question along the principal axes. For a random direction, speciﬁed by radius vector r, we have rij = (sij )−1/2 . In accordance with the Neumann principle (which states that the symmetry group of a certain physical property of a crystal must include the symmetry elements of the point group of the crystal), the symmetry of the characteristic surface corresponds to the symmetry of the physical property. For all positive values of sii the characteristic surface is a sphere for cubic crystals which belong to the highest symmetry category. The characteristic surface of the crystals which belong to the medium category, those with tetragonal, hexagonal or trigonal structures, has the shape of spheroid (prolate or oblate ellipsoid), whereas

168

CHARACTER OF GROUP REPRESENTATION MATRIX

crystals of the lowest symmetry category which are orthorhombic, monoclinic, or triclinic, are described by a characteristic surface in the form of a three-axis ellipsoid. An example of a characteristic surface associated with optical anisotropy represents the dependence of the refractive index n on the direction in the crystal; depending on the shape of this surface crystals are classiﬁed as optically isotropic, uniaxial crystals or biaxial crystals. The main property of the characteristic surface may be stated as follows: if vectors A and B are interconnected by the relation Bi = sij Aj and the radius vector r of the characteristic surface tensor sij is parallel to the vector A, then the direction of the vector B coincides with the normal to the plane, which is tangent to the characteristic surface at the contact point of the vector r. Characteristic surfaces apply in the linear or harmonic response range of physical properties. Besides the characteristic surface, the concept of an indicating surface is sometimes introduced: x12 s12

x2 x2 + 22 + 32 = 1. s2 s3

Radius vectors, which terminate at this surface, designate the absolute values of the physical properties in a given direction. CHARACTER OF GROUP REPRESENTATION MATRIX

The trace or sum of the diagonal elements of a group representation matrix. The character is independent of the choice of coordinate system, and all irreducible representations of the same class have the same character. The character table of the irreducible representations has orthogonality properties (see Group theory). CHARGE CARRIER DRIFT See Current carrier drift. CHARGE COUPLED DEVICES

A broad class of devices (charge transfer devices, charge coupling devices, and related chargeinjection devices) that allows for the scanning of an optical image in a manner similar that of a cathode ray tube (vidicon). The main purpose of such devices is the transmission of TV signals of various spectral bands: they are also used

in random-access memories. The mechanism of charge coupling action can, to some extent, be represented by a combination of a bipolar transistor (motion of minority current carriers) and a eld-effect transistor (controls carrier motion by changing displacement voltage at the gate). The electrodes (gates) have a mosaic structure, and the distance between the edges of adjacent elements does not exceed the diffusion length of nonequilibrium carriers. The application of a bias voltage to a single gate element creates a “potential well” under this element for minority carriers. The latter accumulate under the gate in quantities proportional to their rate of generation. In a two-dimensional array of such elements, each “operating element” with the bias that corresponds to the accumulation of minority carriers has unbiased elements as neighbors on every side. Upon supplying the bias to an element adjacent to the operating one, a “potential well” appears under it. If the well is deep enough the packet of minority carriers from the “operating element” well moves into it. The sequence of voltage pulses at the gate elements is set so that the packet shifts by the length of one element with each pulse, thus the charge of every “operating” element can be led sequentially through to the output element, producing an output signal proportional to this charge. CHARGE DENSITY OSCILLATIONS See Plasma oscillations. CHARGE DENSITY WAVE in metals

Periodic redistribution of electronic, ionic and total charge in space, caused by small periodic displacements of ions near their equilibrium positions in the crystal lattice. The charge density wave (CDW) state is detected via the scattering of X-rays, fast electrons and neutrons, which exhibits diffraction peaks from the source lattice and weaker peaks from their “satellites” (see X-ray structure analysis, Electron diffraction analysis). A charge density wave can appear when the metal is cooled below some critical temperature. The phase transition to the CDW state is characterized by changes in the temperature dependence of the resistance, Hall constant, magnetic susceptibility, and a modiﬁcation of the electronic spectrum of the metal. The charge density wave

CHARGED PARTICLE ENERGY LOSS

period can be commensurate with the period of the source lattice, and in these cases one can talk about commensurate CDWs which differ from incommensurate ones. As a rule in the cases of incommensurability the lattice period depends on the temperature, and structural transitions to the commensurable CDW are possible. The transition to a charge density wave state is found in metals with strong anisotropy of the electronic spectrum. This anisotropy can have a two-dimensional character, when the electrons move freely in a plane (their Wannier wave functions at different points overlap), but between the planes their motion is restricted (due to the weak overlapping of the electronic Wannier functions). Related to such compounds are, e.g., the layered compounds of dichalcogenides of transition metals like TaS2 , NbSe2 (see Quasi-two-dimensional crystals). Anisotropy of a one-dimensional type is realized in compounds with a chain structure, e.g., in organic conductors (see Quasi-one-dimensional crystals). The origin of transitions to the CDW state for all these systems is associated with the features of the geometry of the Fermi surface. The theory shows that if sufﬁciently large sections of this surface are nested, meaning that they are can be overlapped with each other by translation along a reciprocal lattice vector Q, then the polarizability of the system of electrons in the periodic electric ﬁeld of the lattice E = Re (E0 eiQr ) (r is the radius-vector of the lattice point) is high and the lattice becomes unstable with respect to the appearance of periodic distortions with wave vector Q. The distortions are formed below the critical temperature and cause an energy gap to appear in the electronic spectrum at the nested sections of the Fermi surface, i.e. with the complete or partial loss of metallic properties. The degree of nesting, as well as the extent of the metallic property loss grows with increasing anisotropy of the electronic spectrum. In quasi-two-dimensional (layered) compounds the appearance of an energy gap at the whole Fermi surface is impossible, and they preserve their metallic properties at transitions to CDW state, or in case of large displacements of atoms they become semimetals. In quasi-one-dimensional compounds the region of Fermi surface nesting is more extensive, and the

169

energy gap may occur on the whole Fermi surface. Then quasi-one-dimensional compounds in a state with a charge density wave become insulators (see Peierls transition). CHARGE DENSITY WAVE IN SUPERCONDUCTOR See Superconductor with charge (spin) density waves. CHARGED PARTICLE ENERGY LOSS in a solid

This loss occurs during the interaction of incoming charged particles with atoms and electrons of a target. It is characterized by the average braking ability equal to −dE/dx, where E is the particle energy and coordinate x is its initial direction, and by straggling of the charged particle energy loss (by the root mean square scattering of the energy loss value). This energy loss determines the values of charged particle path in the material. Calculation of the energy loss is a complex many-particle problem, and to solve it requires the adoption of a series of approximations which differ for high- and low-energy particles, for long-range and short-range collisions, and also for the different correlations of masses and charges of interacting particles, taking into account the so-called density effect associated with the polarization of the medium by the ionizing particle, of the resonance recharging of the moving ions, etc. The main mechanisms of charged particle energy loss are the nuclear decelleration or braking caused by elastic collisions (taking place without variation of internal energy), collisions of atoms (ions); electron braking caused by the inelastic collisions leading to the excitation and ionization of the atomic electron shells, and also of the free electrons of the irradiated material (see Characteristic energy loss). Besides, there is the charged particle energy loss from radiation – Bremsstrahlung and Cherenkov radiation; the loss is substantial for light particles, especially for electrons and positrons. The value of this loss depends on the energy, charge, and mass of the moving particles, as well as on the charge, mass, and density of the target atoms. For motion close to the direction of low-index crystallographic axes and planes, the energy loss strongly depends on the direction of the incident beam (see Orientation effects; Channeling); in other cases the target may

170

CHARGED PARTICLE PATHS

be approximately considered as an amorphous one with isotropic loss. In the approximation of the Lindhard–Scharf–Schiott theory charged particle energy loss of ions in an amorphous medium is expressed in terms of dimensionless variables for the energy ε = aEM2 /[e2 Z1 Z2 (M1 + M2 )], and coordinate ρ = 4πxa 2 NM1 M2 /(M1 + M2 )2 , where M and Z are the masses and atomic numbers of the incident ions (subscript 1) and of the atoms of the medium (subscript 2), N is the density of the atoms of the medium, 2/3 2/3 a = 0.8853aB (Z1 + Z2 )−1/2 , aB is the Bohr radius. Taking into account the structure of the atomic electron shells supplements the results of the Lindhard–Scharf–Schiott theory concerning an oscillating (within limits of tens of percents) dependence of dE/dx on Z2 caused by the contribution of the valence atomic shells to the charged particle energy loss of the electrons. The charged particle energy losses of positrons and electrons of not too high energies E < Ecr when the role of braking radiation is not yet appreciable, are determined by nuclear and electron braking, with values having qualitative regularities close to the charged particle energy loss of ions, but differing from the ion values mainly due to the mass difference between the electrons (taking into account relativistic corrections) and ions. The value of Ecr may be evaluated from the correlation Z2 Ecr [MeV] ≈ 800. For different energy ranges, masses, particle charges, and target parameters, there are different approximations for the calculation of the charged particle energy loss, and there are also many available experimental data. CHARGED PARTICLE PATHS in condensed media

Characteristics of charged particle trajectories that are limited by the charged particle energy loss during collisions with atoms and electrons of the medium. The particle path in a medium is a broken line since each collision results in a change of particle momentum and direction. The total vector path, R, is the distance between the particle entry point and its terminal point where it has already expended most of its energy and stopped. The projective path Rp presents a projection of R onto the direction x of the initial

particle momentum (e.g., the latter may be normal to the bombarded plane, yz). The transverse path R⊥ characterizes the change of the initial coordinate of the particle in the yz plane at the time the particle stops. Finally, one may consider the total or effective path RL which is equal to the full length of the distance travelled by the particle taking into account all deviations from a linear track. The number of particle collisions per unit path length, the impact parameters for each collision, and, hence, the trajectory of each individual particle are probability variables, even for identical initial conditions of particle motion, so there exists a certain distribution of charged particle paths over their lengths. When bombarding a sample with a beam of ions of the same chemical element with equal initial energies the proﬁle of stopped ions appears to exhibit a certain broadening. Such a distribution is often characterized by the moments M1 = Rp = x; M2 =

Rp2 = (x − x)2 , . . . , Mk = (x − x)k (k = 3, 4, . . .), x k = (r cos θ)k p(r, θ; E) dr, where p(r, θ; E) is the probability for a particle entering the crystal with energy E at the zero coordinate point along the direction n to stop at point r, so that θ = arccos(nr/r). The value

Rp presents the statistical average scatter (straggling) of particle paths, M3 that is a measure of distribution asymmetry. The accepted measure of asymmetry is the so-called distribution skewness, 3/2 Sk = M3 /M2 . In the case of Sk < 0, the path distribution falls off more sharply from its maximum in the bulk sample, and when Sk > 0 a sharper fall-off is at the surface of the sample. The pathways become longer in the case of channeling. Electron pathways in the medium typically feature much sharper trajectory breaks compared to the pathways of heavy particles. Because of multiple collisions, the electron quite soon “forgets” its initial direction of propagation. Moreover, electrons penetrate the medium in a diffusion manner. To retrieve the pathways experimentally electrons of varying initial energies are shot through thin plates. The maximum plate thickness at which a throughput electron current is still recorded corresponds to the maximum path length for an electron with a given energy penetrating the material. A normal pathway is one with a plate thickness

CHEMICAL BONDS

such that the initial electron beam intensity decays by a factor of 6 when passing through it. An empirical dependence for electrons with initial energies E 0.6 MeV is Rp [mg/cm2 ] = 526E[MeV] − 94. CHARGE, MAGNETIC See Magnetic charge. CHARGE-TRANSFER COMPLEXES

Organic compounds consisting of molecules of two types: one acts as an electron donor and the other as an electron acceptor, the charge being redistributed between the neighboring donors and acceptors. Charge-transfer complexes have an electric dipole moment even if they are created from nonpolar molecules, and they exhibit paramagnetic properties, whereas the initial donor and acceptor molecules are diamagnetic. If an electron in the ground state of the organic solid is completely transferred from donor to acceptor, such a compound is called an ion-radical salt (limiting bond case in charge-transfer complexes). Besides weak charge-transfer complexes of ion-radical salts, there are many such compounds with intermediate strength bonds. The properties of chargetransfer complexes are strongly dependent on the extent of charge transfer, and on the magnitude of the donor–acceptor interaction. The electrical conductivity of these complexes at room temperature varies over a wide range: from 10−15 up to 102 –103 −1 ·cm−1 . The temperature dependence of the electrical conductivity is of the semiconductor type; hence, most charge-transfer complexes are organic semiconductors. These are exempliﬁed by compounds of different molecules with the molecular acceptor tetracyanoquinodimethane (TCNQ). Because of the strong acceptor properties, the planar structure, and the high symmetry of the TCNQ molecule, one can obtain charge-transfer complexes with a rather high conductivity (as high as 104 −1 ·cm−1 ). A large variety of organic charge-transfer complexes have been synthesized that exhibit properties ranging from those of semiconductors to metals and superconductors (see Superconductivity). The latter two categories include mainly ion-radical salts. Molecular charge-transfer complexes are of interest as photosemiconductors (see Photoconductivity).

171

CHEMICAL BOND PREDISSOCIATION The state of a chemical bond, usually an ex-

cited one, having an energy that exceeds the energy of atoms in the dissociated state. The latter is separated from the initial state by a barrier which may be overcome by tunneling (see Tunneling phenomena in solids). The simplest example of chemical bond predissociation is the excited hydrogen molecule H2 with a dissociation energy ≈4.4 eV, whereas the excitation energy upon transition of one of the atoms to the level 2p is ∼10 eV. Another example is the state of an α-particle in a radioactive nucleus, e.g., of Ra or U, whose average lifetime is, respectively, 1600 and 4.4·109 years. CHEMICAL BONDS in solids

Bonds between atoms of a solid; isolated atoms decrease their free energy during the redistribution of their electron densities when they join together through chemical bonding. The nature of a chemical bond is determined by the nature of the constituent atoms, and by the type of structure adapted by the solid. There exist molecular crystals, whose structural elements are molecules; under evaporation this crystal type decomposes into molecules. Crystals can be formed from monatomic molecules of noble gases (He, Ne, Ar, Kr, Xe, Rn), diatomic molecules (H2 , O2 , NO, CO), triatomic molecules (H2 O, H2 S, NO2 ), and molecules of a more complex composition (NH3 , CH4 , etc.). In these cases every molecule has saturated bonds, and the attraction of molecules toward each other is through van der Waals forces or hydrogen bonds, as in H2 O, H2 S, NH3 . A certain (additional) role is played by Coulomb forces, if the atoms have a partial charge, as, e.g., in CO2 and H2 O molecules. In cases when the molecules contain atoms of Groups I, II, III, together with those of Groups V, VI, VII of the periodic table, i.e. they are polar molecules, then Coulomb forces become dominant to the extent that individual molecules are not observed in the crystal, and its structural elements are ions. Typical examples are provided by alkali-halide crystals, and oxides of alkaline earth metals. In these compounds every ion is usually symmetrically surrounded by ions of opposite sign (six for FCC NaCl, eight for BCC CsCl); and the stronger ionic bond is formed. For these cases the

172

CHEMICAL DIFFUSION

action of van der Waals forces between ions becomes of secondary importance. The opposite case is provided by crystals of elements of Group IV: diamond, silicon, germanium, gray tin. There are no charges on the atoms of these crystals, and the formation of covalent bonds, or homopolar bonds, is due to the sp3 -hybridization of orbitals (atomic orbitals), and to the attraction of electrons to the nuclei (skeletons) of neighboring atoms. As only four hybrid orbitals may be formed by a combination of s- and p-orbitals, the number of closest neighbors (coordination number) for these crystals is limited to four. Each atom of one sublattice is tetrahedrally surrounded by four atoms of the other sublattice. The binary A(n) B(8−n) type crystallization of elements (sphalerite lattice) is formed analogously, e.g., BN, GaP, ZnS, HgTe, CuCl. However, the atoms of the metal and the metalloid in these compounds possess fractional charges of opposite sign, with the metal atom positively charged. This is a combined (hybrid) polar-covalent bond (ionic-covalent bond). The smaller the number n of the periodic table group, the more ionic the bond. In metals and alloys the so-called metallic bond also occurs: it is formed through delocalization of valence electrons. At the formation of the crystal the outer (valence) s- and p-electrons (elements of Groups I to III, and transition elements) leave their atomic nuclei and migrate between ions over the entire lattice. As this takes place, their kinetic energy decreases (in accordance with the uncertainty relation). It is this energy decrease that is responsible for the formation of a metallic bond; alkali metals and alkaline earth metals possess relatively weak metallic bonds (1 to 2 free electrons per atom), whereas elements such as Fe, Ti, Pt exhibit rather strong metallic bonds. For a fairly broad class of hydrogen-containing organic compounds there is a noticeable contribution to the crystal formation energy from hydrogen bonds. Typical examples are provided by ice, solid ammonia, and the ferroelectric crystal KH2 PO4 . Because of its comparatively small mass, a positively charged hydrogen atom exhibits quantum behaviour and spends some time near an electronegative atom (see Electronegativity) of one of the neighboring molecules, which results in a decrease of the overall system energy. Many solids

exhibit several types of chemical bonds, usually with one or two bonding types dominant. CHEMICAL DIFFUSION The same as Heterodiffusion. CHEMICAL HEAT TREATMENT Heat treatment in a chemically active medium

involves the diffusive saturation of a metal surface with chemical elements of the medium. Both nonmetals (B, C, N, etc.) and metals (Al, Ti, Cr, Zn, etc.) are used as diffusible elements. In a number of cases simultaneous saturation with metals and nonmetals is used, including multicomponent saturation. During chemical heat treatment a diffusion layer is formed as a result of prior processes of dissociation in the active external medium, adsorption of dissociated atoms on the surface of the base metal, and diffusion of the saturating element. Chemical reactions bring about dissociation with the generation of active atomic states of chemical elements (e.g., ammonia decomposition under nitriding). Adsorption of dissociated atoms may take place either through the action of van der Waals forces of attraction, with the generation of an adsorption layer (physical adsorption), or because of chemical bonding with atoms of a metal surface (chemisorption). Simultaneously with these processes, the main chemical heat treatment process goes on, namely the diffusion of adsorbed atoms into the depth of the metal. The result is the formation of a diffusion layer with a certain distribution of diffusible elements relative to the depth. The concentration changes monotonically with depth, so a continuous sequence of solid solutions forms with the base metal. The chemical composition of the layer is more complicated if the solid solutions have limited solubility, or if chemical compounds form. In this case the layer includes different phases, in accordance with the phase diagram of the saturating element with the base metal at the diffusive saturation temperature, and the concentration dependence on the depth can undergo abrupt changes. The duration of diffusive saturation is determined by the depth of the diffusion layer, which increases quadratically with time. The main methods of chemical heat treatment with respect to the type of active medium are: saturation from powders and

CHEMICAL SHIFT

pastes, gaseous media, melts of metals and salts, as well as evaporation of the diffusible element in vacuo. Chemical heat treatment involving a single element includes nitriding, aluminizing, boronizing, siliconizing, titanizing, zinc plating, cementation. Saturation with two elements takes place at aluminoboronizing, aluminosiliconizing, chromosiliconizing, nitrocementation, cyaniding. This treatment involving several diffusible elements includes saturation with boron and silicon together with other metals (Ti, Cr, Mo, W, etc.), as well as saturation with aluminum and chromium together with other metals (Ti, V, Mn, Zn, etc.). Chemical heat treatment is used in industry to increase the reliability and service life of metallic working parts of devices and engines. Depending on the chemical composition of the metallic work piece and the nature of the saturating elements, treated articles may acquire increased hardness, strength, corrosion resistance and cavitation resistance, wear resistance (see Wear), etc. CHEMICAL METHODS OF ANALYSIS

Methods of analysis based on the use of chemical reactions. Methods of quantitative analysis involve the determination of the masses of the reaction products (gravimetry); determination of the volume of the solution of one substance required to react quantitatively with a given solution volume of another substance (titration analysis), determination of thermal effects of the reaction (calorimetry), of its rate (kinetic methods), etc. Methods of qualitative analysis are based on carrying out chemical reactions, which indicate either the presence of ions of certain type in the solution, or the presence of certain atoms in organic compounds. Chemical methods of analysis have been largely superseded by more accurate physical and physicochemical methods of analysis. CHEMICAL POTENTIAL (introduced by J.W. Gibbs, 1873–1878)

Thermodynamic state function, which deﬁnes the change of thermodynamic potential for the change in the number of particles of the ith type Ni in open multicomponent systems with varying numbers of particles, which are described by the grand canonical distribution (see Gibbs distributions). The chemical potential μ of the ith

173

component equals the partial derivative of every thermodynamic potential (e.g., Helmholtz free energy F ) with respect to Ni while holding other thermodynamic quantities constant (e.g., μi = ∂F /∂Ni at T = const, V = const and Nj = const for j = i). The chemical potential for constant pressure conditions is closely related to Gibbs free

energy G = i μi Ni , and in the case of a singlecomponent system μ = G/N , i.e. the chemical potential is equal to Gibbs energy per particle. For quantum systems of bosons, which obey Bose–Einstein statistics, the chemical potential is negative at temperatures higher than the Bose– Einstein condensation temperature T0 , and is equal to zero below T0 , and in systems with varying numbers of particles (phonons in solids, photons in equilibrium with thermal radiation). For a system of fermions, which obey Fermi–Dirac statistics, the chemical potential is positive at temperatures below the degeneracy temperature (Fermi temperature) TF , it coincides with the Fermi energy EF at absolute zero of temperature; and for T > TF the chemical potential satisﬁes the inequality μ < EF . In external potential ﬁelds (gravitational, electric) the role of the chemical potential is played by the quantity μi = μ0i + Ui (r) = const, where μ0i is the chemical potential in the absence of the ﬁeld, and Ui (r) is the potential energy of particles of the ith type in the external ﬁeld. For charged particles in an electrostatic ﬁeld E = −∇ϕ(r) the expression for the electrochemical potential μi = μ0i +ei ϕ(r) = const holds true. Equal values of chemical potential in different phases deﬁne equilibrium conditions for phase equilibria (the so-called Gibbs’ phase rule) and chemical reactions. The chemical potential in a solid determines the electronic work function of a crystal for e ld electron emission, thermionic emission and photoelectron emission, electron af nity, contact potential difference, and other properties. CHEMICAL SHIFT

Term used to describe changes (depending on the speciﬁc nature of the material under investigation) of the positions of energy levels or spectral lines which can arise from the local electronic or chemical environment. The values of chemical

174

CHEMILUMINESCENCE

shifts are usually given as parameters corresponding to the spectrum (energy state) of a given material. Generally the chemical shift is measured either in the same units as the basic quantities which characterize the spectrum, or in dimensionless units. The term is most widely used in high resolution nuclear magnetic resonance (NMR) spectroscopy, in Mössbauer spectroscopy, in the physics of semiconductors to describe the location of impurity energy levels, etc. In high-resolution NMR the chemical shift is the shift of the resonance signal. The mechanism producing this shift is as follows: an atom (molecule) is placed in an applied magnetic ﬁeld B 0 ; and as a result of Larmor precession of electrons oriented parallel to and antiparallel to B 0 the ﬁeld B ∗ arises (see Diamagnetism), so the nucleus experiences the action of an effective magnetic ﬁeld B = B0 − B ∗ = B0 (1 − σ ), where σ is called the screening constant; usually σ ∼ 10−6 . For nuclei of a given type, which are in different electronic surroundings, i.e. either in different molecules or at nonequivalent sites of one molecule, the resonance will be observed for different values of B0 (at a given frequency). In practice the NMR chemical shift is measured in relative units δ = (B − Bst )·106 /B0 , where B and Bst are the respective resonance values of the external ﬁeld for the sample under investigation and a standard substance. The chemical shift is one of the main characteristics of high resolution NMR spectra, which are observed for liquids (and occasionally gases). The value of this shift provides information on the electronic structure of molecules, and the nature of chemical bonds. The development of a recent trend in spectroscopy, namely highresolution NMR spectroscopy of solids, permits the measurement of chemical shifts in solids. In the Mössbauer effect the chemical shift (also called isomer shift) makes its appearance if the source and absorber differ chemically. In the physics of semiconductors a chemical shift manifests itself in the difference between the energy states of impurity levels, expressed in terms of the effective mass, and the energy states calculated from theory, taking into account corrections to the potential due to the speciﬁc atom (ion). For example, some donor levels exhibit fairly large

chemical shifts in their ground state energies due to correlation and exchange effects involving the donor and core electrons. CHEMILUMINESCENCE Luminescent excitation that results from chem-

ical reactions. The process of chemiluminescence involves the emission of radiation either by products of a chemical reaction, or by other components which become excited by absorbing energy transferred to them from reaction products. Chemiluminescence in solids arises at a boundary with a gaseous or liquid phase as a result of heterogeneous reactions (see Heterogeneous system), which proceed either spontaneously (intrinsic chemiluminescence) or under action of various external factors: e.g., electrical, electrolysis (electroluminescence). A speciﬁc case of chemiluminescence is bioluminescence (e.g., luminescence of rotten wood). Chemiluminescence constitutes the basis of action of chemical lasers, and is used for the analysis of gases and solid surfaces. CHEMISORPTION, chemical adsorption

Chemical binding of particles of a substance (atoms, molecules, radicals) by a solid surface. It differs from physical adsorption by its stronger bonding, that is by a higher value of the binding energy (0.5–10 eV). The bond between the adsorbed particle and the solid can have both covalent and ionic components; the former due to overlap of the electronic wave functions of the adsorbed particle and the substrate atoms, and the latter due to the transfer of charge from the adsorbed particle to the solid material. An adsorbed ion in conjunction with charges which screen it can form a dipole, which results in the adsorbed ﬁlm changing the electronic work function of the solid. Particles chemically adsorbed on the surface of a solid interact with one another, and sometimes generate an ordered two-dimensional lattice of adatoms (see Monolayer). Chemisorption plays an important role in the oxidation of metals, heterogeneous catalysis, crystal growth, electronics, etc. CHEMISTRY See Crystal chemistry, High-energy chemistry, Mechanochemistry, Mesonic chemistry, Quantum chemistry, Radiation chemistry, Solid state chemistry.

CHIRALITY OF MAGNETIC BUBBLE DOMAINS

CHERENKOV RADIATION (S.P. Vavilov, P.A. Cherenkov, 1934); referred to as Vavilov–Cherenkov radiation in the Russian literature Photons emitted by charged particles moving

in a medium with a speed v which exceeds the speed of light u = c/n in this medium, where n is the refractive index. In condensed matter with high values of n Cherenkov radiation is observed at electron energies of about 105 eV, and at protons energies of 108 eV. This radiation is explained via Huygens principle by noting that waves which are emitted at points along the charged particle trajectory for the condition v > u will overtake waves emitted earlier by the particle. As a result of their interference, a light cone is formed having a vertex that coincides with the instantaneous position of the emitting particle, with θ the angle between the direction of the particle’s movement and the direction of propagation of the outgoing radiated wave satisfying the relation cos θ =

1c . nv

The spectral distribution of energy E(ω) for Cherenkov radiation is determined by the relation dE c2 e2 = 2ω 1− 2 2 dω c v n for the condition v > c/n(ω). There is no radiation for frequencies ω which do not satisfy the above condition. Cherenkov radiation has found wide application in Cherenkov counters used for determining the speeds, charges, and masses of fast charged particles (electrons, positrons, mesons, protons, and antiprotons); and for studying optically anisotropic media, including waveguides. CHI PHASE (χ -phase) An intermetallic compound with a cubic lattice

isomorphic to that of cubic α-Mn. It is formed mainly by transition metals. The best known chi phases are those involving rhenium with refractory materials. In alloys of rhenium with molybdenum, tungsten, niobium and tantalum the chi phase contains about 75 at.% Re. In the systems Mo–Re and W–Re the chi phase is obtained by the peritectic reaction (see Peritectic alloys) at 1850 ◦ C

175

in the system Mo–Re and at 2150 ◦ C in the system W–Re; and this reaction only takes place for a narrow region of homogeneity. In the systems Nb–Re and Ta–Re the χ -phase melts without decomposition and exhibits a broad range of homogeneity. In systems formed by Re with Ti, Zr and Hf the composition of the χ -phase is approximately Me5 Re24 ; it is formed by the peritectic reaction, and has a moderate range of homogeneity (Me–Ti, Zr or Hf). The chi phase has also been observed in binary systems Al–Re, Nb–Os, Tc–Zr. Chi phases are assumed to be “electron compounds” (see Hume-Rothery phases). A number of chi phases transform to the superconducting state, with the highest transition temperature Tc = 12.9 K for Nb0.24 Tc0.76 (see Superconducting intermetallic compounds). CHIRALITY (fr. Gr. χειρ , hand)

Handedness, or belonging to one of two (“lefthand” or “right-hand”) non-superimposable mirror image conﬁgurations. See also Enantiomorphism. CHIRALITY IN LIQUID CRYSTALS

Absence of planes of symmetry in the molecules of liquid crystals. Chirality in liquid crystals leads to instability of a uniform (homogeneous) state, and the formation of spatially-periodic (spiral) structures (right-handed or left-handed) in some liquid crystal phases (cholesteric liquid crystals, blue phases, smectic liquid crystals of the C type); see Chirality, Enantiomorphism. CHIRALITY OF MAGNETIC BUBBLE DOMAINS The sign of the relative rotation of the magnetization in the center of a domain wall for a magnetic bubble domain with topological index S = 1, which does not contain Bloch lines. The magnetization in a magnetic domain wall is ei-

ther aligned along the vector tangent to the lateral surface of a domain wall, or is opposed to it. Hence two possible states of a magnetic bubble domain, labeled χ ± , are more favorable (in the context of magnetostatics) than all other states. By convention the label χ + is assigned to a clockwise rotation of the magnetization when observing along the rotation axis direction. The twisting deﬂections of χ + and χ − are equal in magnitude.

176

CHOLESTERIC LIQUID CRYSTAL

It should be noted that, by virtue of domain wall twisting, the above deﬁnition is valid only for the cross-section of the magnetic bubble domain by a plane that is at equal distances from the magnetic lm surfaces. Transitions between the χ + and χ − states of magnetization rotation usually occur when horizontal Bloch lines are present. CHOLESTERIC LIQUID CRYSTAL, cholesteric, chiral nematic, cholesteric phase (fr. Gr. χoλη , bile, σ τ ερεoς , solid, and χειρ , hand) An analog of a nematic phase (see Nematic liquid crystal) for a material containing chiral mole-

cules, that is molecules which differ from their mirror image structures (see Chirality in liquid crystals). When chiral molecules are dissolved in a nematic liquid the structure undergoes a helical distortion to form a helical phase called a cholesteric. This phase was originally observed in the ethers of cholesterol, hence its name. A cholesteric, like a nematic, lacks long-range order, and the molecular orientation has a preferred axis denoted by a director n which is perpendicular to the helical z axis. The local symmetry is close to ∞22 (or C∞h ), with the spatial distribution of the apex positions of the director vector n tracing out a spiral or helix. The spatial period or step along the helical axis is one half the pitch of the spiral because director orientations n and −n are equivalent, as is the case in nematics. The step of the spiral L depends on the chemical composition and on the temperature, and typical values lie in the range from 350 nm to 650 nm, corresponding to visible and near UV wavelengths. Cholesteric liquid crystals possess unique optical properties such as Bragg diffraction of light beams at the spiral structure, enhanced optical activity, etc. These properties are widely used in various ﬁelds of engineering, in particular in the medical area. CHRISTOFFEL SYMBOLS (E.B. Christoffel, 1869)

The Christoffel symbol is Γkli = g in Γn,kl , where the metric tensor gik deﬁnes Γi,k,l = (∂k gil + ∂l gki − ∂i gkl )/2, and ∂i = ∂/∂x i . The Christoffel symbols do not form a tensor; in particular by choosing a particular system of coordinates one may reduce all the Christoffel symbols to zero at any given point. In curvilinear coordinates in a

ﬂat space the Christoffel symbols are used to form covariant derivatives of tensors. These symbols are used in elasticity theory to characterize changes of the basis vectors ei of the local coordinate system deformed together with the body: dei = Γkil el dx k . Christoffel symbols and gik are both expressed through the strain tensor uik : gik = δik + 2uik (δik is the unit tensor), Γi,kl = ∂k uil + ∂l uki − ∂i ukl . To take into account dislocations and internal stresses, the Christoffel symbols are replaced, within the framework of the mechanics of solids, by the coefﬁcients of linear (afﬁnity) coherence, Γikl . The number of independent values of Γikl is equal to 15 (in contrast to 9 for the previous case). Γikl may be separated into symmetric (Γi(kl) ) and antisymmetric (Γi[kl] ) parts with respect to the indices k, l: Γikl = Γi(kl) + Γi[kl] . The quantity Γi(kl) characterizes the pure deformation of the trihedron deﬁned by the basis vectors ei , and Γi[kl] characterizes the rotation of the trihedron during its transition from point to point. The quantity Γi[kl] is directly linked to the density of dislocations in the material; the sum of the Burgers vectors of dislocations passing through a small area S is proportional to the convolution of the tensor of the area S and Γi[kl] . CHROME PLATING

Application of chromium coatings to the surface of materials to increase their hardness, wear resistance (see Wear), corrosion resistance and friction resistance, and also for decorative purposes. The thickness of the coatings varies from 1 μm to 3 mm, their hardness ranges from 500 to 1200 kg/mm2 . Electrolytic chrome plating is carried out from aqueous chromium-oxide solutions either with a sublayer of copper and nickel, or without it. The appearance, structure, physicochemical and mechanical properties of the coatings may be changed by variation of the electrolyte composition, and the method of electrolysis. Also in some areas of engineering diffusion chrome plating is used, preferably from the lowest halide compounds of chromium, by means of thermal decomposition or reduction in a gaseous, solid or liquid medium, with successive diffusion of chromium into the depth of the parts being coated.

CINNABAR

CHROMIUM, Cr

A chemical element of Group VI of the periodic table with atomic number 24 and atomic mass 51.996. There are four stable isotopes: 50 Cr, 52 Cr, 53 Cr, 54 Cr. The outer shell electronic conﬁguration is 3d 5 4s 1 . Successive ionization energies are 6.764, 16.49, 31, 51, 73, 90.6 eV. Atomic radius is 0.125 nm; radius of Cr2+ ion is 0.084 nm, of Cr3+ is 0.063 nm. Covalent radius is 0.118 nm. Oxidation states are +2, +3, +6. Electronegativity is 1.55. Under normal conditions chromium is a silvery-white metal. The crystal lattice is body¯ (O 9 ), with centered cubic, space group I m3m h parameter a = 0.28848 nm (at 298 K). Density 3 is 7.194 g/cm (at 298 K); Tmelting = 2176 K, Tboiling = 2742 K. Heat of melting is ≈14.0 kJ/mole, heat of evaporation is 393.34 kJ/mole; speciﬁc heat is 460 J·kg−1 ·K−1 (at 298 K). Debye temperature is 630 K. Linear thermal expansion coefﬁcient is ≈6.5·10−6 K−1 (at 298 K); coefﬁcient of thermal conductivity is 67 W·m−1 ·K−1 (at 298 K). Adiabatic elastic moduli c11 = 350.0, c12 = 67.8, c44 = 100.8 (in GPa). Young’s modulus is 279.65 GPa (at 298 K); shear modulus is 102.02 GPa (at 298 K), Poisson ratio is 0.31. Ultimate strength is 84 MPa (at 298 K, after recrystallization). Relative elongation is 0% (at 298 K, after recrystallization). Vickers hardness is 100 to 200 HV. Linear lowtemperature electronic speciﬁc heat coefﬁcient is 1.4 mJ·mole−1 ·K−2 . Electrical resistivity is 129 n·m. Temperature coefﬁcient of electrical resistance is 3·10−3 K−1 (293 to 373 K). Hall constant is 3.63·10−10 m3 /C (at 293 K). Coefﬁcient of absolute thermal electromotive force is 16.2 μV/C. Chromium is an antiferromagnet with Néel temperature TN = 311 K. Molar magnetic susceptibility is 3.6·10−6 CGS units. Nuclear magnetic moment is 0.474 nuclear magnetons. Reﬂection coefﬁcient of 500 nm wavelength light is 67%. Electronic work function of polycrystal is 4.68 eV. Chromium is employed to give glass an emerald green color, and it ﬁnds wide use as a catalyst. CHROMIUM ALLOYS Chromium-based alloys. Doping Cr with small additions (up to 1%) of yttrium, rare-earth elements and titanium causes the binding of these

177

atoms into refractory compounds (see Refractory materials), and reﬁning the metal matrix decreases the cold brittleness temperature slightly, and increases its plasticity. At the same time the corrosion resistance increases. Strong doping of Cr with iron, cobalt, nickel, ruthenium, and rhenium changes the electronic structure of chromium, and in some cases its crystal structure and phase composition. It provides for an appreciable decrease of the cold brittleness temperature. However, in such a case alloy brittleness appears, due to the formation of a sigma phase. Chromium alloys are smelted in archer or induction furnaces in an inert gas atmosphere, or fabricated by the method of powder metallurgy. A thermomechanical treatment of low-doped chromium alloys, when a ﬁnegrained and cellular dislocation structure arises (see Cellular structure), permits an increase of the strength and, at the same time, the cold brittleness temperature. Low-doped chromium alloys are used as thermal-environment resistant materials, and as high-temperature materials at 1000–1100 ◦ C, with a short-term heating capability up to 1500–1600 ◦ C. Highly-doped alloys are used in the chemical engineering industry, in the production of components for magnetohydrodynamic generators, foundry castings, etc. CINNABAR (fr. Gr. κινναβαρι), HgS A mineral, the red-colored stable modiﬁcation of mercury sulﬁde. The Mohs hardness is

2–2.5, and the density is 8.0–8.2 g/cm3 ; the crystal family is trigonal, and the space group is P 31 21 (D34 ), a = 0.4146 nm, c = 0.9497 nm. Another modiﬁcation of mercury sulﬁde, black metacinnabarite with the ZnS type structure, is unstable and gradually transforms into cinnabar. This most important mercury mineral is used to produce the metal. Artiﬁcially, cinnabar is prepared by rubbing mercury with sulfur with subsequent treatment with alkalis. The heat of formation equals −59 kJ/mol (at T = 298 K). Cinnabar exhibits a high volatility (t sublimation = 580 ◦ C). The crystal lattice energy is 3,578 kJ/mol. The crystals are composed of polymer chains –Hg–S–Hg–S– with the parameters: d(HgS) = 0.236 nm, ∠HgSHg = 105◦ , ∠SHgS = 172◦ . Artiﬁcial cinnabar is a semiconductor material used for photoresistors, as a catalyst, and as a pigment.

178

CIRCULAR PHOTOVOLTAIC EFFECT

CIRCULAR PHOTOVOLTAIC EFFECT Photovoltaic effect observed in doubly refracting crystals (see Gyrotropic media) illuminated by circularly or elliptically polarized light (see Polarization of light). There is a difference between

the circular photovoltaic effect and other photovoltaic effects: the resulting current is proportional to the degree of circular polarization of the radiation Pcirc and changes its direction in accordance with the sign of the polarization. The “circular” photovoltaic effect for elliptically polarized light is described by the following relation: jα = γαβ i[E × E ∗ ]β , where j is the current density, and E is the amplitude of the light electric ﬁeld (see also Bulk photovoltaic effect). For circular polarization this becomes i[E × E ∗ ] = |E|2 Pcirc q/q, where q is the wave vector of the light. Initially the circular photovoltaic effect was observed in tellurium, then it was studied in a variety of crystals including a number of ferroelectrics. The origin of this effect arises from the asymmetry of the distribution of the electrons excited by the light. This asymmetry is due to the correlation between the electron angular momentum (spin) and its linear momentum in gyrotropic crystals. The inverse effect, the so-called optical activity (see Rotation of light polarization plane) induced by the current and resulting from the spin orientation during the current ﬂow, has also been observed in tellurium. In nongyrotropic crystals, which possess no center of symmetry, the circular photovoltaic effect does not occur, while the phenomenon of optical activity may appear from uniaxial deformation or an applied magnetic ﬁeld. Such a magneto-induced circular galvanomagnetic effect was observed in p-type GaAs. In crystals of low symmetry, including those possessing a center of symmetry, the circular drag effect described by the relation jα = Tαβγ i[E × E ∗ ]β qγ may be observed. In contrast to the circular photovoltaic effect, the circular drag effect is due to the transfer of phonon momentum to the electrons. The current in this effect changes its sign, not only when the

sign of the circular polarization changes, but also when the light propagation direction changes. The circular photovoltaic effect may used in inertialess receivers of polarized laser radiation, in elements of optical memory on photorefractive crystals (see Photorefraction), and also as a mechanism of fourwave mixing of isofrequency waves in various nonlinear optical frequency converters. CLATHRATE COMPOUNDS (fr. Gr. κληθρα , adler-tree) Phases comprising at least two compounds,

with the molecules of one enclosed in the molecular voids or lattice cavities of the other. They bear a close similarity to interstitial solid solutions. As a rule, only van der Waals forces act between the molecules of a clathrate compound. The binding energy of each enclosed molecule is about ≈50 kJ/mol. This relatively high value for van der Waals interaction is explained by the molecule and void geometry ﬁtting well into one another, and by the many points of bonding by the molecule. Depending on the void type, clathrate compounds are categorized as lattice or molecular types. Lattice clathrate compounds can only be solids, and are further classiﬁed by the shape of their voids as channel, cage (originally only this type was termed clathrate), and laminated varieties. Examples of “host” compounds that form cage clathrates are uria, thiouria, hydroquinone, phtalocyanines, etc. There is a wide range of corresponding “guest” compounds: hydrocarbons, alcohols, many gases. Cyclic molecules usually form the molecular clathrate compounds, such as cyclodextrin and other macrocyclic compounds. Compounds of relatively small dimensions can be enclosed in the voids of such “hosts”. The clathrate compounds exhibit, in the general case, a variable composition. They are employed mainly to isolate and purify “guest” molecules. CLAUSIUS–MOSSOTTI EQUATION (R. Clausius, O. Mossotti, 1879)

Relation between the relative (dimensionless) dielectric constant of isotropic nonpolar insulators, ε(ω), at a frequency ω (see Temporal dielectric dispersion) and the polarizability, α(ω), of the atoms that make up the crystal lattice:

α(ω)N ε(ω) − 1 = , 3ε0 ε(ω) + 2

(1)

CLOSE-PACKED STRUCTURES

where N is the number of atoms per unit volume, and SI units are used. This expression is sometimes written in terms of the electric susceptibility χ(ω) = ε(ω) − 1. If the square of the refractive index, n(ω), in the transparency region is substituted for ε(ω) then Eq. (1) is called the Lorentz–Lorenz relation. Eq. (1) differs from the frequently used expression ε = 1 + αN/ε0 which is applicable in the case of a linear response of a medium (crystal) to a macroscopic electric ﬁeld averaged over the medium, since the Clausius–Mossotti equation is derived taking into account the local electric ﬁeld that acts on an atom in the crystal, and this differs from its mean value. The Clausius–Mossotti equation for cubic crystals coincides with the expression for ε derived from the rigorous Ewald method. See also Langevin–Debye equation.

179

Fig. 1. Planar triangular close packing arrangement of spheres.

CLEMENTI FUNCTION (E. Clementi)

A wave function of a certain nl-shell of an atom (or ion) whose radial part is represented as a superposition of Slater functions (see Slater rules), the parameters of the latter being derived from minimizing the total energy of a given multielectron state. Clementi functions can be used as the ﬁrst approximation for a non-empirical computation of crystals. CLOSE-PACKED STRUCTURES, closest-packed structures

Geometrical arrangement of rigid spheres of the same radius, which provides the densest ﬁlling of space. There is only one way of attaining such a conﬁguration in a plane, which consists in arranging a lattice (the sites formed by the centers of balls) based on an equilateral triangle conﬁguration, as shown in Fig. 1. The threedimensional closest-packed sphere structure is constructed from the above planar arrangement by superimposing layers, one onto another, in such a way that the upper layer of a pair lies with its atoms set in the recesses of the layer below; the density of√packing (packing fraction) in this case being π/ 18 ≈ 0.74. There are two ways to do this, and either one is effectively equivalent. The third layer also has two possibilities, but they are not equivalent. One way for positioning the third layer is to place its spheres in recesses between second layer atoms that are not directly above the

Fig. 2. Three-dimensional close packing arrangements of spheres: (a) face-centered cubic, and (b) hexagonal close-packed.

atoms of the ﬁrst layer, and this gives what is called an ABC arrangement of layers, as shown in Fig. 2(a). None of the three layers is directly above another. Another way to position the third layer is with its atoms in recesses directly above the ﬁrst layer, thereby forming what is called the ABA sequence of layers, as shown in Fig. 2(b). Each subsequent layer can be positioned in one of two ways, leading to an inﬁnity of possible closest packed structures if the number of layers becomes very large, and the sequencing of the A, B, and C type layers is random subject to the condition that two identical layers cannot be adjacent to each other. If the sequence is a periodic one, then the corresponding closest-packed sphere structure is spoken of as periodic highest-density spherical packing. According to the Belov theorem, periodic closest-packed sphere structures may exhibit only eight different space groups of symmetry: P 3m1, R3m, P 3m1, R3m, P 6m2, P 63 mc, P 63 /mmc, F m3m. The packing consisting of only two alternating layers ABAB. . . is referred to as highest-

180

CLOSE PACKING, RANDOM

density hexagonal packing or hexagonal closepacked (HCP). The three-layered ABCABC. . . arrangement is given the name highest-density cubic packing or cubic close packing (CCP or FCC). The centers of the spheres of the latter structure form a face-centered cubic lattice. The tendency of atoms to attain closest packing results in the fact that most metallic atoms crystallize in one of the close-packed arrays which is almost always the hexagonal (e.g., Mg, Nd, Zn) or the facecentered cubic (e.g., Ag, Al, Cu) one. In addition bulky components (e.g., anions oxygen or sulfur) of various widely occurring chemical compounds also form close-packed arrays, and the diversity of structures stems from the fact that there are many ways of arranging the smaller cations throughout the smaller tetrahedral and larger octahedral cavities of the closest-packed structure. CLOSE PACKING, RANDOM See Random close-packing model. CLUSTER

A stable aggregation or group of atoms or molecules distinguished by certain physical or chemical features from other similar stable microobjects. Several particles constitute the lower limit on the size of a cluster, while the upper limit can often be deduced from one of the following two traits: (1) the addition of one more particle to the aggregation appreciably affects the system properties; or, (2) the number of particles at the surface, i.e. those which differ in properties from the bulk due to their proximity to the surface, is comparable to the total number of internal particles in the cluster. These conditions usually limit the number of particles in a cluster to the range 102 –103 . Larger agglomerates of particles in a material are called phase precipitates. Examples of clusters are: agglomerations of impurity atoms or intrinsic defects (see pile-up of dislocations and point defect clustering) arising in the bulk of a solid due to their mutual attraction and to the diffusion of particles (during the growth of crystals or during heat treatment), under the action of external energetic particles (see Collision cascade and Subcascades), under the action of light (in photographic emulsions), etc. The atomic or molecular

aggregates that comprise a small particle can be formed during the coagulation of particles, e.g., those dispersed in air (aerosol particles), during the sputtering of materials under ion bombardment or other high-energy factors, during evaporation, etc. Surface clusters can be formed by deposition of particles on the surface of a solid. The stability of a cluster can depend on the number n of constituent particles, and sometimes it depends on whether n is odd or even. Thus it was established by means of mass spectrometry that when Li atoms are evaporated into an inert gas an appreciable amount of Li2 , Li6 and Li8 appears, whereas Li3 , Li5 , Li7 , and Li9 are either entirely absent, or are present in only trace amounts. During the ion sputtering of Ag crystals three times more Agn clusters form with odd n compared to the number with even n. A method termed the cluster approximation is often employed in numerical computations of the energy spectra of ideal crystals, or of crystals with defects, with a cluster deﬁned here as a lattice of a ﬁnite number of atoms. Atom–atom potentials and cluster boundary conditions are chosen to provide for a high cluster symmetry, for correct values of the crystal lattice constants, and for stability. Systems of particles can also have fractal properties (see Fractal) arising from special rules followed in building the system. For instance, a percolation cluster is a set of certain lattice sites obtained by successive translations of a given length from an arbitrarily chosen starting site to other randomly chosen sites; the dimensions of such a cluster are not limited to integers (see Percolation theory). In quantum scattering theory coupled states of several particles are termed clusters; with every cluster considered as a separate scattering channel. CLUSTER APPROXIMATION

The breaking down of a system into subsystems (see Cluster) that interact weakly with each other. This approximation is employed in thermodynamics, statistical physics, and quantum scattering theory. It involves expressing the wave function of a multiparticle system far away from the scattering region as a superposition of states corresponding to individual isolated particles and/or groups of them. The cluster approximation in the

COADSORPTION

theory of lattice defects in crystals is based on singling out a region in the crystal that incorporates the defect and several coordination spheres surrounding it. The local defect properties (binding energy, energy level position, wave function of the localized state, lattice conﬁguration) are then computed over this region using one of the standard molecular theory methods. The interaction of the cluster with the rest of the crystal is accounted for by using a self-consistent eld approach. Sometimes the term cluster approximation is employed to designate an approximate method for computing the parameters of an ideal crystal by representing the crystal as a cluster consisting of a relatively small number of atoms. Certain boundary conditions are imposed upon the outermost atoms to ensure the stability of such a conﬁguration. See also Watson sphere. CLUSTER, CYBOTAXIC See Cybotaxic clusters. CLUSTER DEPOSITION

Formation of heterogeneous lm s composed of clusters of particles. The ﬁlms form via the deposition from a ﬂow of clusters, e.g., produced by ion sputtering of different targets, or by homogeneous gas phase nucleation, or due to a heterogeneous nucleation at the substrate surface. A cluster may contain from several to a few thousand particles. An assortment of cluster deposition technology methods provides a range of structures and cluster properties which determine the ﬁlm formation kinetics and ﬁlm properties. Using the method of cluster deposition at low temperature one can obtain the epitaxial deposition of multicomponent compounds such as semiconductors, or one can grow diamond-like carbon lms, oxides, nitrides, carbides, etc. CLUSTER, NONCRYSTALLINE See Noncrystalline clusters. CLUSTER SPUTTERING Sputtering of a solid under the action of ion bombardment during conditions when clusters of

different size composed of the solid’s own atoms plus impurity atoms are predominant in the ﬂux or ﬂow of sputtered material. Not only neutral

181

clusters, but also positive and negative ions, polyatomic and molecular ions and their fragments, are found in the sputtered ﬂux during the cluster sputtering of metals, semiconductors, insulators, organic compounds, polymers and biomolecules. The mass-spectra of sputtered clusters range from dimers through aggregates of tens and hundreds of atoms, up to large bioorganic molecules and their clusters. The energy distribution of sputtered clusters reaches 100–200 eV, the average being 2–10 eV per cluster of ions and 10–20 eV for neutral clusters. The sputtering probability sharply drops with an increase in the number of atoms in the cluster, and it can undergo oscillations associated with the binding energy. In particular, there may be less charged metallic clusters having an even number of atoms than those having an odd one. The mechanisms of the cluster sputtering of solids are not yet understood. Theories of direct knock-out (for small clusters), of recombination, and of shock waves, have been proposed to explain the phenomenon. The latter theory allows for the emergence of large clusters and of complete bioorganic molecules (such as insulin) under the impact of a single heavy accelerated ion, or of a fragment from nuclear ﬁssion. Cluster sputtering plays an important role in secondary ion mass-spectrometry, and it also ﬁnds applications in designing sources for accelerated cluster and macromolecular ion formation, including ionized bioorganic molecules. COADSORPTION

A cooperative adsorption of adsorbates of differing chemical composition. In the case of physisorption the mutual inﬂuence of these adsorbates is associated with the difference in the heats of adsorption, which may result in the particles with a greater heat of adsorption driving out those with lesser heats of adsorption. In the case of chemisorption, the mutual effects of the adsorption of different species is associated with the formation of chemical bonds of the adsorbates with the substrate; this can result in a promotion or inhibition of the sorptional activities of neighboring centers. Such an inﬂuence may stretch over the distance of several lattice constants, and may result in the emergence of not only a short-range, but also a long-range order. The phenomenon of

182

COAGULATION

heterogeneous catalysis is based on the process of coadsorption of molecules of differing chemical composition.

COAGULATION

See Coalescence.

COAL

Carbonaceous porous combustible stratiﬁed rock; with a surface of fracture which is either lustrous or lusterless. Coal contains a maximum of 30% of incombustible components (ash). Coal is formed by carbonization (metamorphic transformation) of the remains of decomposed plants under prolonged exposure to temperature, ionizing radiation of natural radionuclides, etc. According to the degree of carbonization, brown coal (lignite) and black coal are distinguished. The carbon content increases from ∼65% (by mass of organic components of coal) for soft lignites to >91% for anthracites; accordingly, the oxygen content decreases from 30 to 2%, and the hydrogen content decreases from 8 to 91% C exhibit an abrupt increase of aromaticity, and an abrupt decrease of electric resistance. Coals contain paramagnetic centers, with concentration reaching 1020 spin/g.

COALESCENCE (fr. Lat. coalesco, grow together, be coupled) The spontaneous merger of small particles of

a solid that results in the formation of a single larger particle whose shape minimizes its free energy. The phenomenon of the formation of pores in a solid is also known. The coalescence of particles may occur in sols, aerosols, and on the surface of a solid. Coalescence is distinct from coagulation, the latter being the mere sticking together of colliding particles. Coalescence is associated with diffusion processes that take place under the inﬂuence of surface tension forces. It will be slowed down by charged particles. Surface coalescence is conditioned by strains in the substrate, by its surface roughness, and by its polycrystalline structure. COATING

Application of a layer, which has protecting, decorating, conducting, etc., properties, to the surface of a material. Metals and alloys, as well as nonmetallic substances, are used as coating materials. Application of a metallic coat is performed through hard facing with a thin layer of salts in oil (baking coating), chemical deposition, galvanization (electrolytic deposition, see Electroplating), dip coating (dipping into melted metal or into aqueous salt solutions in the presence of oxygen), vacuum evaporation, cathode sputtering (sprayed metal coating), etc. Nonmetallic coats (varnishes, enamel and oil paints) are applied to surfaces through brushing, spraying under pressure, fusion. Colloid mixtures of graphite with varnish, or of a metal with varnish, are used as nonmetallic conducting coatings. Anodic oxidation is used in order to coat the surface with an oxide lm ; carbon ﬁlms are obtained through decomposition of a dried layer of carbonic acid through heating to 473 K, or high vacuum evaporation. COATING, ANTICORROSIVE See Anticorrosive coatings. COBALT (Lat. cobaltum ), Co

Chemical element of Group VIII of the periodic system with atomic number 27 and atomic mass 58.9332. The naturally occurring stable isotope 59 Co is very close to 100% abundant. The

COERCIVE FORCE

most important artiﬁcial isotope is radioactive 60 Co with a half-life of 5.24 years. The outer shell electronic conﬁguration is 3d 7 4s 2 . Successive ionization energies are 7.865, 17.06, and 33.50 eV; electronegativity is 1.7. Atomic radius equals 0.125 nm; the Co2+ ionic radius equals 0.072 nm, that of Co3+ is 0.063 nm. The oxidation state is +2, +3, rarely, +1 and +4. Cobalt in the free state is a metal of silver-steel color. It exists in two polymorphic conﬁgurations: α-Co with a hexagonal close-packed lattice (space 4 ), a = 0.2507 nm and c = group P 63 /mmc (D6h 0.40686 nm at 298 K), and β-Co with a facecentered cubic lattice (space group F m3m (Oh5 ), a = 0.3548 nm). The temperature of the start of the transformation of α-Co into β-Co by heating is 750 K; the temperature of the start of the reverse transformation by cooling is 676 K. The density of α-Co is 8,183.6 g/cm3 (at 293 K), that of β-Co is 8,739 g/cm3 (at 298 K), the binding energy is −4.387 eV/atom at 0 K and −4.4 eV/atom at room temperature; T melting = 1768 K, T boiling = 3203 K. The heat of fusion is 16.2 kJ/mol. The speciﬁc heat is 414 J·kg−1 ·K−1 at standard pressure and temperature. The Debye temperature is 385 K. The coefﬁcient of linear thermal expansion parallel to the c axis is 14.62·10−6 K−1 , and perpendicular to the c axis, it is 10.96·10−6 K−1 . The thermal conductivity is 142 W·m−1 ·K−1 at 163 K and 70.9 W·m−1 ·K−1 at 290 K; the adiabatic elastic rigidity coefﬁcients of α-Co crystal are: c11 = 306.28, c12 = 165.12, c13 = 101.9, c44 = 75.33, and c33 = 357.4 GPa at 298 K. Young’s modulus of α-Co is 220.9 GPa, that of β-Co is 199.7 GPa; the modulus of rigidity of α-Co is 84.5 GPa, that of β-Co is 74.7 GPa; Poisson ratio of α-Co is 0.307, and that of β-Co is 0.337 (at 298 K). The ultimate tensile strength is 260 MPa (at 298 K), and the relative extension is 5% (at 293 K). The Brinell hardness is 124 MPa for cobalt subjected to 1.2–3 GPa treatment. The self-diffusion coefﬁcient equals 5.91·10−26 m2 /s. The Sommerfeld low-temperature electronic speciﬁc heat coefﬁcient (linear term) equals 4.73 mJ·mol−1 ·K−2 . Electrical conductivity is 55.7 n·m (at 293 K); the temperature coefﬁcient of electric resistance equals 604·10−5 K−1 . The Hall coefﬁcient is

183

0.36·109 m3 /C. The absolute thermal electromotive force coefﬁcient equals 18.5·10−6 V/K. The optical reﬂectivity for 5.0 μm wavelength is 92.9%. The work function for a polycrystal equals 4.41 eV. Cobalt is a ferromagnet with Curie point T C = 1393 K. The nuclear magnetic moment of 59 Co equals 4.639 nuclear magnetons, and the atomic magnetic moment equals 1.715 Bohr magnetons. The thermal neutron absorption crosssection is 34.8 barn. Cobalt ﬁnds its use as a component of hard magnetic, corrosion resistant and high-temperature alloys and coatings, as well for glass dyeing; the intermetallic compound SmCo5 is used for the fabrication of permanent magnets (see Samarium– cobalt magnet), and radioactive 60 Co is employed in medicine as a source of γ -radiation. COERCITIMETER

Device for measuring the coercive force or coercivity Bc of magnetic materials. The most common types are coercitimeters for coercive force measurement by magnetization MBc or by induction BBc . For an MBc measurement the sample is magnetized to saturation and then demagnetized up to the point of zero magnetization, and the magnetic ﬁeld strength that brings this about corresponds to MBc . For measuring Bc by induction the sample is made part of a closed magnetic circuit, and the strength of the demagnetization ﬁeld at which the induction B in the sample goes to zero is accepted as the value Bc (i.e., BBc ). For small values of the coercive force MBc ≈ BBc . See Magnetometry, Magnetic structure analysis. COERCIVE FORCE, coercive e ld, coercivity (fr. Lat. coercitio, con nement)

Value of an applied magnetic ﬁeld Bc which reduces the magnetization of a magnetized magnetic substance to zero. In many magnetic materials the magnetization process is not reversible, but takes place around a hysteresis loop. An applied magnetic ﬁeld Bm produces a state of magnetization Mm in the material. The removal of the applied ﬁeld does not reduce the magnetization to zero, but rather to the remanent magnetization value Mrem . A reverse direction ﬁeld −Bc must be applied to reduce the magnetization to zero. Increasing the reversed applied ﬁeld to −Bm induces the reversed magnetization −Mm , and most

184

COHERENCE

of a hysteresis loop is thereby traced out. When Bm is small the coercive ﬁeld Bc is also small, where of course Bc < Bm , and increases in Bm cause Bc to increase. Very large applied ﬁelds Bm induce a saturation magnetization Ms , so further increases in Bm have no effect. The coercive ﬁeld Bc measured at saturation is called the coercivity, and the associated hysteresis loop is called an extremal hysteresis loop. The coercivity of various materials varies over a very wide range from 10−4 mT to 10 T. (Some authors deﬁne Hc = Bc /μ0 , where 1 mT ∼ = 795.8 A/m.) The coercivity arises from the back magnetization process, and involves the magnetic anisotropy energy, the magnetostriction, and the saturation magnetization. In a particular material the coercivity can differ considerably depending on its structural state; it depends also on the direction in anisotropic materials, on the temperature, and on the presence of external stresses. The extremal coercivity value for a given material equals its anisotropy ﬁeld and can be achieved, e.g., in ﬁne monocrystal ferromagnetic single-domain particles, in which back magnetization is brought about by irreversible rotation of the spontaneous magnetization vector. High coercivity values can be obtained in close to perfect crystals where, near saturation, the formation and growth of back magnetization nuclei are impeded. In most ferromagnets the coercivity is determined by the critical ﬁeld for irreversible displacement of magnetic domain walls, and this can be impeded by various inhomogeneities such as internal stress gradients, foreign inclusions, structural defects, and so on. COHERENCE See Macroscopic quantum coherence, Structural coherence. COHERENCE FACTORS

Renormalization coefﬁcients F 1,2 (k, k ) appearing in the Bardeen–Cooper–Schrieffer theory (BCS theory) which connect the matrix elements B1 (k , s | k, s) for single-particle transitions k, s → k , s in the system of non-interacting Bogolyubov quasi-particles (see Bogolyubov method), and the matrix elements B2 (k , s | −k, −s) for the processes of the annihilation of quasiparticle pairs in the states k , s and −k, −s. The

latter appear in a superconductor under the effect of an external perturbation with corresponding matrix elements B0 (k , s | k, s) for the singleelectron transitions k, s → k , s in the normal state of a metal: B1,2 = F1,2 B0 . According to the BCS theory, F1 (k, k ) = Uk Uk ± Vk Vk , F2 (k, k ) = Uk Vk ± Uk Vk , where the Uk , Vk are the Bogolyubov transformation coefﬁcients (see Canonical transformation method), with the sign determined by the nature of the external perturbation. Coherence factors are needed for theoretical descriptions of the different kinetics in superconductors associated with transitions in the system of Bogolyubov quasi-particles. This provides, e.g., in the BCS theory, an explanation of the difference between the type of temperature dependence of the nuclear spin relaxation time and that of the coefﬁcient of ultrasound adsorption in a superconductor. COHERENCE LENGTH in superconductors

Length scale for the variation of the order parameter (see Ginzburg–Landau theory of superconductivity) ξ0 , ξ(T ) = √ 2(1 − T /Tc )1/2

ξ0 =

vF , πΔ0

where v F is the Fermi velocity, Δ0 = E g /2 is the superconducting energy gap at T = 0, and T c is the critical temperature of the second-order phase transition from the normal to the superconducting state. According to the scale invariance hypothesis, at the point T = T c the coherence length ξ goes to inﬁnity as ξ(T ) ∼ (1 − T /T c )−ν . The critical index is ν = 1/2 in the self-consistent e ld approximation. The coherence length also determines the effective size of Cooper pairs with the binding energy 2Δ. In pure superconductors with T c ≈ 1–10 K, for T T c , ξ is equal to ξ0 ≈ 10−5 –10−4 cm in order of magnitude. In “dirty” superconductors with short electron mean free paths l ξ(T ) the effective coherence length is ξ eff ∼ = (ξ l)1/2 . In highly disordered superconducting alloys (compounds) and in amorphous superconductors ξ 10−6 cm, which provides

COHERENT BREMSSTRAHLUNG

185

high values of the Ginzburg–Landau parameter κ = λ/ξ and the upper critical eld B c2 (T ), where λ is the magnetic ﬁeld penetration depth. COHERENT BREMSSTRAHLUNG A type of Bremsstrahlung (braking radiation) speciﬁc for monocrystals. The Bremsstrahlung of

charged particles in single crystals at high particle energies effectively differs from that of an isolated atom. For relativistic particles (total energy E far exceeds rest energy, Lorentz factor γ = [1 − (v/c)2 ]−1/2 E/(m0 c2 ) 1), there is a formation zone one radiation length l long in which the Bremsstrahlung process takes place which can substantially exceed an atomic size, i.e. the creation of a radiated photon takes a long enough a time so that a particle can traverse a macroscopic distance. The time of photon generation is long compared with the duration of a particle’s impact upon a nucleus, therefore the process characteristics are determined mainly by interference during the radiation process, rather than by the nature of the collision with an individual nucleus. The formation zone in monocrystals may be substantially longer than the separations between the atoms of the crystal lattice. In this case all the atoms in the zone take part in the process of coherent radiation, with the Bremsstrahlung intensity in monocrystal increasing, relative to that of an an amorphous substance, proportional to the number of atoms located in this zone: N eff ∝

l 2E(E − ω) ∝ . a m2 c3 ωa

The presence of interference in the monocrystal Bremsstrahlung arises from simple kinematic considerations. Suppose a particle entering a crystal at a small angle, θ , relative to a crystallographic axis encounters atoms along its path spaced a distance a/θ apart (a is the lattice constant), and subsequent acts of Bremsstrahlung emission take place. Suppose the energy of the radiation of quanta is small, and the radiation only weakly affects the particle motion (its momentum is virtually unchanged at radiation). The quanta are emitted mainly in the forward direction of the particle motion (within a cone whose angle is inversely proportional to the Lorentz factor γ ). If t0 is the time of emission at the ﬁrst atom, the

Intensity I of Bremsstrahlung of electrons in a diamond single crystal as a function of the energy ω of the emitted quanta at the incidence angle θ = 4.6 mrad relative to the (110) axis (an electron beam of initial energy 1 GeV is directed along the (001) plane); shown are theoretical calculations (solid lines) and experimental data (dots).

Bremsstrahlung emission at the second atom will occur at the time t0 + a/(vθ). As the ﬁrst emitted quantum reaches the second atom at the moment t0 + a/(cθ), the phase difference between the two must be equal to 2πn (where n is an integer) for the interference to amplify the radiation: a 1 1 = 2πn. − ω θ v c With a ﬁxed particle energy, E, and a ﬁxed magnitude of quantum energy, ω, there is a particular angle θmax at which constructive interference is observed: a , θmax = 2πnl where l is the radiation length. There may be different numbers of lattice sites inside the Bremsstrahlung region, depending on the angle of incidence of the charged particle relative to the crystallographic planes or axes, which results in an appearance of maxima and minima in the Bremsstrahlung spectrum presented as a function of the angle at which fast particles enter the monocrystal. The intensity of coherent Bremsstrahlung in the Born approximation is proportional to the square of the number of atoms within the radiation length. If the Born approximation is inapplicable, the dependence of coherent emission intensity I on the number of atoms

186

COHERENT CHANNELING

within the formation zone is weaker, having a logarithmic dependence (see Fig.). The coherent Bremsstrahlung exhibits a rather high degree of polarization, and this results in intense beams of polarized γ -quanta being produced by electron accelerators. COHERENT CHANNELING See Okorokov effect. COHERENT CONDENSATE See Bose condensate. COHERENT POTENTIAL METHOD (P. Soven, D. Taylor, 1967)

An analogue of the mean ﬁeld method used for computing the electronic structure and electronic properties of disordered alloys (see Disordered solids) based on the formalism of multiple scattering theory. The applicability of this method is not related to limitations on the magnitude of the impurity scattering potential, or of the alloy component ratios. A scattering matrix (t -matrix) is assigned to each individual atom in this approach. Systems of atoms are described on the basis of the scattering characteristics of individual atoms using a Green’s function that depends upon the positions of the scattering atoms. It is assumed that the energy spectrum of the ensemble as a whole can be “macroscopically” described with the mean Green’s function −1 G(z) = z − ε(k) − (z) ,

k

where k (z) is a self-energy term (see Mass operator of quantum mechanics), and ε(k) is the dispersion law for an electron in an unperturbed translationally-invariant crystal. To complete the Green’s function deﬁnition, the system is presumed to behave as if one and the same coherent potential, σ (z), is assigned to each lattice site, and an effective potential, w n = wn − σ (E), is introduced for every site to replace the random potential energy of an electron wn (see Random potential). The self-consistency condition is taken as follows: w n = 0. tn = 1−w n n|G(z)|n

This implicit equation deﬁnes σ (E) ≡ k (E), and permits the determination of the coherent potential as a function of a spectral variable z. This method is believed to provide one of the best single-site approximations for obtaining the spectral characteristics of disordered systems. The small parameter of the method for the calculation of the energy spectrum is the quantity (a/R0 )3 , where a is a lattice constant, and R0 is a characteristic damping or jump length of the hopping integral. A similar small parameter appears when computing corrections to the expression for the electrical conductivity of a disordered binary alloy within the formalism of the coherent potential method. The physical sense of this parameter can be explained as follows: if a sphere of radius R0 encloses a large number of sites then one can neglect the ﬂuctuations of the number of atoms of both types A and B inside this sphere. COHERENT PRECIPITATES New phases formed at phase boundaries which display a structural coherence there. Coherent

precipitates arise as a result of the decomposition of supersaturated solid solutions (see Alloy decomposition), or from other phase transitions: a martensitic transformation, a eutectic (see Eutectic alloys), etc. Coherent precipitates may be wholly or partially coherent, depending on the type of structural coherence. They form during the early stages of phase transformations; later on, the structural coherence will be destroyed due to structural dislocations which form at the phase interface to make the precipitates non-coherent. The appearance of coherent precipitates with an appreciable mismatch of crystal lattice constants δ = (a p − a m )/a m , where a p and a m are lattice constants of the precipitate and matrix, respectively, gives rise to coherent elastic stresses, and to an increase of the elastic energy of the system by a magnitude εe ∝ δ 2 . That results in an increase of the strength of an alloy, of its coercive force, and of the magnetostatic energy (see Magnetostatics). In aging alloys (see Alloy aging), the elastic interaction of coherent precipitates may produce modulated structures. Coherence disruption, and an appearance of non-coherent precipitates, will usually result in deterioration of the alloy strength characteristics.

COLD BRITTLENESS

COHERENT SCATTERING REGIONS Largest regions of a crystal from which elastic scattering of radiation (X-rays, neutrons, etc.) by individual atoms or unit cells is coherent. The di-

mension D of a coherent scattering region can be deﬁned as the distance at which the phase shift of the waves scattered by atoms (cells) reaches π as compared to an ideal crystal. The value of D depends on the reﬂection indices hkl of the planes. In the case of an ideal mosaic crystal, D coincides with the size l of mosaic blocks. Provided the disorientation of adjacent blocks is ψ λ/ l (λ is the radiation wavelength), the value of D may be estimated from the width δθ of the X-ray line at its half-height: D ≈ λ/( θ · sin θ B ), where θ B is the Bragg angle. In the opposite case (when ψ λ/ l), the regions of coherent scattering may cover several blocks (D ∝ λ/ϕ > l). The blocks of the mosaics do not exclusively determine the range of coherent scattering in a real crystal. Stacking faults (leading to an effective reduction of the coherent scattering regions), small-angle boundaries, degree of uniform bending of crystallites, and internal microstresses in crystallites also play roles. To separate the effect of mosaics from that of microstresses, one may apply harmonic analysis to calculate the normalized Fourier coefﬁcients An in the reﬂection curve (the proﬁle of the X-ray line), P (2θ). The values of An can be written as the product An = An An , where An , An are the contributions from regions of coherent scattering and of microstresses, respectively. In the xyz coordinate system, with xy planes coinciding with reﬂecting planes, one may deﬁne the dependence of An on the reﬂection index 00l and then, extrapolating An (l) to l = 0, ﬁnd An = An (0). The derivatives of An characterize the average size D0 of the coherent scattering region, and the distribution Pn of the regions of coherent scattering transverse and along the z axis direction: −(dAn /dn)n=0 = c/D0 (c is the unit period along the z axis), d2 An /dn2 = Pn . COHESION (fr. Lat. cohaesus , stuck)

Linkage (binding) between two solid bodies of similar chemical composition in contact with each other. It results from a balance between longrange repulsive and short-range attractive forces. The cohesion energy is an important characteristic associated with chemical bonds. It is deﬁned as

187

the work required to move far apart the units of a bound structure. It can be experimentally found by evaporation or sublimation. The largest cohesion energy values are found in condensed phases (liquids and solids) where the chemical bonds are mainly ionic, covalent or metallic in character. The cohesion energy in real gases is several orders of magnitude smaller. The cohesion strength depends on the mutual orientations of the crystal lattices of the bodies in contact, on their geometrical perfection, and on the degree of their surface cleanliness. The cohesion strength is calculated from the expression P = (α10 + α20 − α12 )/a where α10 and α20 are the speciﬁc energies of the surfaces in contact, α12 is the speciﬁc energy of the grain boundary interface, and a is an interatomic distance. If the contacting surfaces are aligned relative to the symmetry elements then α10 = α20 = α, α12 = 0, and Pmax = 2α/a. The actual strength is smaller than Pmax due to the lack of smoothness of an actual contact. Showing up in the cohesion linkage zone are stresses arising from mismatches in the crystal geometry of the surfaces in contact. COINCIDENT-SITE LATTICE An auxiliary lattice considered in the description of particular grain boundaries. A coincident-

site lattice is that sublattice of the complete superposition lattice whose sites are occupied by atoms of both lattices of a bicrystal, i.e. the sites coincide in each of the crystals that are separated by the boundary. The reciprocal relative fraction of coincident sites is designated by Σ . The symmetry of the coincident-site lattice is determined by the symmetry of the pair of conjugated crystals, by the axis of their relative orientation, and by the value of the corresponding rotation angle. See Grain boundary, Grain boundary lattice. COLD BRITTLENESS

The change of the failure mechanism from tough failure to brittle failure (or quasi-brittle failure), which occurs with a decrease of temperature within a comparatively narrow temperature range. This change of failure mechanism involves abrupt reduction of plasticity-related characteristics and strength. According to the Ioffe theory, cold brittleness is the consequence of an abrupt increase of

188

COLD CATHODE

the yield limit σs with decreasing temperature, the temperature dependence of the breaking stress σf being comparatively weak. Cold brittleness occurs below the temperature at which the curves of σs (T ) and σf (T ) versus T intersect. Modern microscopic dislocation theories attribute the sharp temperature dependence of the yield point to the presence of a covalent component in the interatomic bond (see Covalent bond), and to the high value of the Peierls–Nabarro stress (see Peierls– Nabarro model) at the plastic deformation of covalent crystals. Hence the cold brittleness arises due to the abrupt decrease of the mobility of dislocations with decreased temperature, and to the decrease of the rate of stress relaxation at the apexes of cracks and at other stress concentrators (see Stress concentration). The reciprocal of cold brittleness is given the name cold reluctance. This term is descriptive of the ability of materials to retain plasticity and failure toughness with decreasing temperature. The susceptibility of a material to cold brittleness is determined by the cold brittleness temperature (or cold brittleness threshold) Tc . Upper u and T l ) and the lower cold brittleness points (Tcb cb l are commonly distinguished. The lower point Tcb is the minimal deformation temperature at which plastic deformation precedes the failure, and the failure is totally tough in its nature. The value of u depends heavily on the deformation rate ε˙ , Tcb increasing with its increase. Various methods of hardening of materials (raising the dislocation density): solid-solution hardening, dispersion hardening (see Precipitation-hardened materials), etc. l . Only a result in an increase of the value of Tcb reduction of the crystal grain size or the formation of a disoriented dislocation cellular structure can lead to the reduction of Tcb and the improvement of strength properties. As the failure mechanism changes from transcrystalline failure to intercrystalline failure, the cold brittleness temperature may abruptly increase.

ﬁlms, semiconductor ﬁlms, p–n junctions biased in the gate direction (see Semiconductor junction), transistor structures, M–I–S structures (see Metal–insulator–semiconductor structures), M–S structures (M is metal, I is insulator, S is semiconductor), semiconductor structures with a negative electron af nity, etc. COLD ELECTRONS

An electron gas in the conduction band of semiconductors (holes in the valence band) with an average energy ε appreciably less than the thermodynamic equilibrium value ε0 . This phenomenon of electron cooling is due to various mechanisms related to the motion of the current carriers in an electric ﬁeld, or to optical transitions of the charge carriers. For instance, electron cooling will occur if the overall current in a semiconductor is directed opposite to the internal electric ﬁeld in a space charge region, or because of another inhomogeneity of the semiconductor. In electric ﬁelds, where the current is directed along the ﬁeld, a cooling of the carriers is possible when the dominant scattering of the electron energy occurs by optical phonons, and the momentum scattering is by ionized impurities under conditions when the electron–electron interaction is negligible. While acted on by an electric ﬁeld an electron is able to emit an optical phonon, and thereby diminish its energy (i.e. cool), and the scattering by ionized impurities promotes the accumulation of such electrons. Hence it is possible to cool carriers by light through the agency of direct band-to-band transitions. For this purpose it is necessary (when the energy of scattering via interelectron collisions is negligible compared to such scattering of photocarriers by optical phonons) to excite the photoelectrons with a ﬁxed initial energy εi greater than ε0 by utilizing light of such a wavelength that, after the emission of n optical phonons, the photocarriers should have a ﬁnal energy εf < εi . COLD WORKING

COLD CATHODE

Unheated cathode emitting electrons by means of eld emission of electrons. These are e ldemission cathodes, and there are also various types of cathodes emitting nonequilibrium electrons excited by an internal ﬁeld: dispersed metal

Industrial term no longer used much. It means hardening of a metal under the action of cold plastic deformation, but not strain hardening (see also Work hardening). Cold working in optimal mode increases hardness and yield limit, resistance to fatigue deformations, and a decrease of plasticity and

COLLECTIVE EXCITATIONS IN SUPERCONDUCTORS

impact strength. It is used in technology for surface hardening of work pieces with the help of

steel- or cast iron-shot blasting impact treatment, rolling, etc. COLLAPSE OF ELECTRON ORBITS

A sharp decrease of the average radius of an electron orbit in an excited atom occurring for a small change of the nuclear charge (atomic number), Z. The collapse of electron orbits takes place when the screened electrostatic potential −U (r), acting on the electrons and the orbital or “centrifugal” potential 2 l(l + 1)/(2mr 2 ) (where r is the distance from the electron to the nucleus, l is the orbital quantum number, and m is the electronic mass) approximately compensate for each other. Then the effective potential U eff = −U (r) +

2 l(l + 1) 2mr 2

can exhibit two valleys or minima, one near the atom nucleus (at r ≈ a B , where a B is the Bohr radius), and the other at the atom periphery (at r ≈ 10a B ), separated by a positive potential barrier. The deepening of the internal well with increasing Z at a given l results, at a certain critical value of Z = Z c (which depends on l, and also on the electron conﬁguration and on the level), in the redistribution of electric charge density from the outer valley into the inner one, which is interpreted as an electron collapse. This collapse of electron orbits is possible for electrons with l 2. In the isoelectronic sequence of argon-like ions, the collapse of 3d-electrons in the 2p5 3d conﬁguration takes place at Z c = 19, viz., at the transformation from Ar to K+ , while in the isoelectronic sequence of xenon-like atoms the collapse of the 4f -electron in the 3d 9 4f conﬁguration takes place at Z c = 55, i.e. at the transformation from Xe to Cs+ . If the atom or ion is present in a solid then the orbits that did not collapse strongly overlap with neighboring atomic coordination spheres, and the corresponding electrons often become delocalized. Photoabsorption spectra reﬂect the participation of such states, and provide information on the electronic structure of such a solid (see Fine structure of X-ray absorption spectra).

189

COLLECTIVE EXCITATIONS

Motions in a system with a large number of interacting particles associated with the excitation of some collective degrees of freedom, and manifesting themselves in a cooperative dynamics of all the particles (see Phonons). The collective excitations are not necessarily associated with mechanical displacements of the particles: they may be, e.g., electronic excitations in atoms (see Excitons) or excitations of magnetic (spin) degrees of freedom (see Magnons). The collective excitations in condensed media propagate as an ensemble of waves, each of them representing a certain kind of motion characterized by a velocity and an energy. In quantum theory collective excitations are regarded as quasi-particles, their dynamics being described by the corresponding equations of motion. The collective excitations for weak interactions in a system, when the harmonic approximation is valid, obey the superposition principle and play the part of elementary excitations. Introducing the concept of collective excitations facilitates the treatment of a number of physical properties of weakly excited condensed media. Explaining some of these properties requires taking into account the interactions of the collective excitations, which is equivalent to introducing an anharmonicity into their description. In macroscopic systems with a high degree of excitation the collective excitations become transformed, and they can appear as solitary waves (solitons) or shock waves. COLLECTIVE EXCITATIONS IN SUPERCONDUCTORS

Mutually coupled oscillations of the order parameter and of an electric ﬁeld. At a temperature near the critical (transition) temperature, the existence of weakly damped oscillations of this type with an acoustic spectrum is possible. Such oscillations (experimentally discovered by P.L. Carlson and A.M. Goldman in 1975) show up at frequencies which exceed both the reciprocal energy relaxation time, and the reciprocal lag time for the establishment of an equilibrium distribution of quasi-particles over the branches of the energy spectrum. This collective mode represents oscillations of the population differences between the branches of the energy spectrum. Simultaneously, a longitudinal electric ﬁeld appears in the

190

COLLECTIVE VARIABLES METHOD

superconductor, along with currents of normal excitations and of the superconducting condensate directed opposite to one another, so that there is no net current. The phase velocity of such excitations equals: c = [2ΔDχ(2πT τ )]1/2 , where D = v F l/3 is the electron diffusivity (diffusion coefﬁcient), Δ is the energy gap in the superconductor, τ is a characteristic time of scattering from impurities, T is the temperature, χ is the Gorkov function introduced in the theory of superconducting alloys, v F is the Fermi velocity, and l is the electron mean free path. Another type of oscillation existing in superconductors is an oscillation of the order parameter amplitude which has a resonance character (Schmid mode, A. Schmid, 1975). This is associated with the possibility of a virtual decay of Cooper pairs, which requires an energy input of 2Δ. This process involves violation of the energy conservation law and, in accordance with the quantum-mechanical uncertainty principle relating energy and time, must proceed for times of the order of /(2Δ). The amplitude of the order parameter perturbation oscillates with a frequency ω = 2Δ/, and tends toward its steady-state value with a power law dependence on the time. Inelastic scattering mechanisms can bring about an exponential decay of such oscillations. In a hypothetical superconductor treated as a superﬂuid Fermi liquid there are weakly damped oscillations of the phase of the order parameter which have an acoustic spectrum (Anderson– Bogolyubov mode). However, an excitation of the electron density accompanies these oscillations, hence, their frequency is increased up toward the plasma frequency in real superconductors because of Coulomb interactions. COLLECTIVE VARIABLES METHOD

A method of statistical physics that introduces long-range interactions into the thermodynamic and structural properties of multiparticle systems. The description of interacting particles (e.g., atoms, ions or molecules) using collective variables is based on an extended phase space consisting of individual particle coordinates and collective variables associated with the waves of density ﬂuctuations of a certain system parameter (see Fluctuations of atomic positions). Depending on the speciﬁc problem, the latter may be the den-

sity of the number of particles, density of electric charge, spin density, etc. In the simplest case of a single-component system, the collective variables will be deﬁned by means of the Fourier components of the operator of the number density of particles: N 1 exp(ik·r j ), ρ k = √ N j =1

k = 0,

(1)

where r j are the coordinates of the j th particle, and N is their total number. The condition k = 0 √ excludes the constant term ρ k=0 = N δk,0 . The transition to an expanded phase space that includes individual coordinates, {r} = (r 1 , . . . , r N ), and collective variables, {ρk }, is effected via a transfer function which is a product of corresponding δ-functions. Hence, e.g., the system conﬁguration integral can be represented as follows: (2) QN = Q0N (dρ)J (ρ) exp −βθ(ρ) , where Q0N is the conﬁguration integral of the subsystem with short-range interactions, the function 1 (dr) exp −βU0 (ρ) J (ρ) = V N Q0N δ(ρk − ρ k ), (3) × k=0

is the Jacobian of the transition to collective coordinates, the differential factors have the form (dr) =

N j =1

dr j ,

(dρ) =

dρk ,

k=0

where β = 1/(k B T ) is the reciprocal temperature of the system, U0 (r) is the potential energy of the short-range interactions, and the function θ(ρ), given by θ(ρ) =

N N2 ν(k)(ρk ρ−k − 1) + ν(k = 0), V 2V

k=0

(4) is the representation in collective variables of the potential energy of long-range pair inter-particle interactions, ν(k) = dr e−irk Φ(r) is a Fourier component of the long-range potential Φ(r), and V is the system volume.

COLOR CENTERS

A similar transformation to collective variables also can be brought about by means of an integral transform of the Gaussian factor exp[−βθ(ρ)]. The method of collective variables is used to describe the properties of a variety of real systems. Thus, an ion-molecular approach in the theory of electrolytic solutions, based on an equivalent account of the interactions of all the particles in solution, has been developed within the framework of collective variables. This method, supplemented by the density matrix shift transformation, has been successfully employed in the theory of quantum Bose- and Fermi-systems, in particular for constructing a theory of liquid 4 He and describing the electron gas in metals (see Bose–Einstein statistics and Fermi–Dirac statistics). Variables associated with the order parameter of the system have been introduced into the set of collective variables in the theory of secondorder phase transitions, and the explicit form of the transfer Jacobian, J (ρ), is of a non-Gaussian character for three-dimensional systems. In another approach, the collective motions of systems of interacting particles are treated by the canonical transformation method, whereby a transition is made to collective coordinates and momenta that correspond to collective oscillations, or to the elemental excitations associated with them. Since the collective coordinates and momenta are not conventional variables, a transition to them involves additional conditions that conserve the total number of degrees of freedom in the system. COLLISION CASCADE

The avalanche-like process of dislodging (displacement of) atoms (ions) from the sites of a crystal lattice (or of an amorphous solid). The collision cascade arises after energy transfer to the target atom by an external particle as a result of sequential collisions of atoms in the vicinity of the initially displaced one. If the energy of the initially displaced atom is ε, the collision cascade occupies the spatial domain of size l(ε), where l(ε) is the mean free path as a function of its energy. The cascade time is 10−14 –10−13 s; where the cascade over a domain of enhanced concentration of radiative defects arises with its central part enriched with vacancies, and the peripheral one enriched with

191

interstitial atoms. The primary relaxation of a cas-

cade takes ∼10−13 –10−11 s, with some interstitial atoms returning to their initial sites. Then the secondary stage of relaxation occurs, controlled by thermally activated processes (primarily by diffusion). On irradiation with dense beams or with radioactive decay, spatially uniform collision cascades can arise, their only common quantitative characteristic being the cascade function or the radioactive damage function ν(ε). It equals the total number of atoms (ions) displaced from the sites of the solid body lattice by the initial atom with energy ε. Low-energy cascade: ε < εc , where εc is the critical energy, with negligible retardation of the moving atom by electrons below it. All the energy of the atom goes to displace atoms from lattice sites, so that αε (ε < εc ), ν(ε) = εd where εd is the energy for creating a stable vacancy–interstitial atom pair, and α is a factor on the order of unity. As commonly assumed, εd ∼ 25–80 eV, α ∼ 0.4–1. Theoretical values of εc are 0.1 MeV for Fe and 3 MeV for U . For a high-energy cascade: ε > ε c . The retardation of atoms down to energy εc occurs mainly due to electrons of the medium, i.e. without dislodgment of new atoms. Therefore, ν(ε) =

α εc εd

(ε > εc ),

where α is a factor on the order of unity (it can differ somewhat from α). See also Seeger zone. COLLISION IONIZATION See Impact ionization. COLLISION RADIATION See Bremsstrahlung. COLOR CENTERS, F -centers Point defects with optical absorption in the transparent region of a defect-free crystal. Color

centers are related to either impurities (impurity color centers), or intrinsic structural defects in crystals (intrinsic color centers). The main methods to stimulate the formation of color centers are

192

COLORED SYMMETRY

vacancies). Color centers are also found in glasses (see Vitreous state of matter), e.g., a non-bridging oxygen atom in vitreous quartz (band with a maximum at 4.75 eV). The main applications of color centers in practice are lasers, photopigments, dosimetry, and diagnostics of minerals. COLORED SYMMETRY

Color centers.

doping, deviation from stoichiometric composition, and irradiation by ionizing radiation. Electronic transitions that determine the color center absorption are shown schematically in the ﬁgure. Transitions 2 and 3 produce, as a rule, wide absorption bands; transitions 1 give either narrow or broad bands, depending on the magnitude of the electron–phonon interaction. Transitions 4 are observed only under high-power pulse excitation with the aid of time-resolved spectroscopy. Reverse transitions may proceed with photon emission; in this case a color center is simultaneously a luminescent center. Many color centers involve a point defect that has trapped an electron (electron color centers) or a hole (hole color centers). The association of elementary defects (vacancies, interstitial atoms, impurity atoms, or impurity ions) results in the formation of aggregate color centers. An increase in temperature and illumination in the absorption bands of color centers may lead to the release of trapped electrons or holes, i.e. to the destruction (discoloration) of color centers. The most widely studied color centers are in ionic crystals, in particular, in alkali-halide crystals. For example, F -centers (anionic vacancy with a trapped electron, named from the German word “Farbe” for “color”) produce an intense absorption band in the visible region, which corresponds to a transition similar to the 1s–2p transition in a hydrogen atom (F -band), and weaker K-, L-bands refer to transitions to higher F -center excited states. Also H -centers (interstitial atoms of halide X0 ), and Vk -centers (self-localized holes X− 2 ), produce broad bands in the ultraviolet region. In covalent crystals, the absorption of color centers typically occurs as narrow lines, e.g., GR1 and ND1 centers in diamond (neutral and negatively charged

A theory of generalized symmetry of material objects (media and structures), which combines the global symmetry of the system as a whole with the local symmetry of its structural elements. Depending on the method of combination of the groups of global (external) G- and local (internal) P -symmetries, the following colored symmetry groups are distinguished: (1) P -symmetry groups, which are subgroups G(p) ⊆ P × G of the direct products of groups P and G; (2) Q-symmetry groups, which are subgroups G(q) ⊆ P λG of the semidirect products of P and G; (3) Wp -symmetry groups G(Wp ) ⊆ Pwr G = P G × G, which are subgroups of the wreath product (for groups G(Wq ) – of twisted wreath product) of P and G, where P G is the direct product of groups P , taken nG times, n = |G| is the order (or power) of the group G: P G = P g1 × P g2 × · · · × P gn , and the elements gi ∈ G indicate the position of each individual group P in the n-fold direct product. These groups differ in the manner of their effect on a mass point, and in the multiplication law of their elements. In terms of physical interpretation, the lowest groups G(p) and G(q) , isomorphic to the groups G, describe the magnetic exchange symmetry of the structures of magnetically ordered crystals. Groups G(Wp ) and G(Wq ) ↔ G, involving the effect of translation on a mass point (depending on its coordinate), describe the symmetry of real crystals, including quasi-crystals (icosahedral phases), and polysystem molecular crystals with so-called “super-Fedorov” symmetry. COLORED SYMMETRY GROUP

In the general case the subgroups of the direct products (P × G) and the semidirect products (P λG) of groups of external (global) G and internal (local) P symmetries, as well as subgroups of the wreath product Pwr G = P G λG, which operate over subspaces of geometrical coordinates

COMMENSURATE STRUCTURE

193

r ∈ R(3), and of their nongeometrical (“colored”) ◦

counterparts S ∈ S(d). According to the laws of multiplication and to the action of combined elements (p, g) or . . . p(r k ) . . . |g, p ∈ P , p(r k ) ∈ P qk r 1 = P rk ⊂ P r1 × · · · × P rk × · · · = P G of ◦ the material point (S , r), groups of four types are singled out; of global action: ◦ ◦ ◦ P : (p, g) S , r = pS , gr = S , r , (pi , gj )(pk , gl ) = (pi pk , gi gl ) ∈ G(p) ⊂ P × G, ◦ ◦ ◦ Q: (p, g) S , r = pg S , gr = S , r , (pi , gj )(pk , gl ) = pl gj pk gj−1 , gj gl ∈ G(q) ⊂ P λG and of local action – depending on the coordinate ◦

r k = gk r 1 of the point (S , r k ): ◦ ◦ Wp : . . . p(r k ) . . . |g S , r k = p(r k )g S , gr k , . . . pj (r k ) . . . |gj . . . pl (r k ) . . . |gl = . . . pj (r k )pl (r k ) . . . |gl gl , ◦ ◦ Wq : . . . p(r k ) . . . |g S , r k = p(r k )g S , gr k , . . . pj (r k ) . . . |gj . . . pl (r k ) . . . |gl = . . . pj (r k ) gj pl (r k )gj−1 . . . gj gl . The colored symmetry groups are closely connected with the theory of so-called ﬁber SR-spaces (SR ⊂ S(d) × R(3), or SR ⊂ S R (d) × R(3)), and n = (d +3)-dimensional groups, which are their generalized projections onto the threedimensional space. The colored symmetry groups are used to describe magnetically ordered crystals (see Magnetic symmetry group). See also Colored symmetry. COLOR GROUP See Shubnikov groups.

Curves of hardness versus layer depth for different combined heat treatment techniques: nitration or nitrocementation chemical heat treatment (N), and electrocontact (E), induction (I), and laser (L) high-speed hardening.

out, and values of the technological parameters being used. Multiple combined heat treatment techniques allow the variation of properties corresponding to different requirements for surface layers and internal bulk (core) material. Schematic curves of hardness as a function of layer depth are presented in Fig. as an example, where the lower solid curve is a thermo-chemical treatment employing nitration or nitrocementation (N), and the remaining curves represent high-speed hardening via electrocontact (E), induction (I), and laser (L) processes. It is possible to improve hardness and other mechanical properties in near-surface regions, and depending on the methods of heating, at different distances from the surface, taking into account structure and microstructure variations. It is also possible to obtain gradients of particular properties needed for speciﬁc loading conditions. As examples of how metals can undergo combined heat treatments we refer to prior quenching with tempering before thermo-chemical treatment at low temperatures; cementation; nitrocementation with hardening, etc. COMMENSURABLE STRUCTURE See Commensurate structure.

COMBINED HEAT TREATMENT

COMMENSURATE STRUCTURE, commensurable structure

The heat treatment of materials including combinations of heat with chemical and mechanical modes. The choice of combined techniques takes into account the loading conditions, detailed geometry, sequence of operations being carried

A long-period structure, which arises from periodic distortions of an initial lattice due to displacements of atoms from equilibrium positions. The commensurate structure is generally formed during lowering of the temperature at a phase

194

COMPACTION

transition. In a number of cases the system undergoes a sequence of phase transitions to various commensurate states (with sequential variations of the superlattice constant), until reaching the ﬁnal commensurate phase which has a period a that is a multiple of the initial lattice constant a, i.e a = na, where n is an integer (so-called “devil’s staircase”). The transition from the initial structure to a commensurate one proceeds in certain materials through an intermediate temperature incommensurate structure, with a superstructure constant incommensurate with the lattice constant of the initial phase (see incommensurate–commensurate phase transition). The commensurate structure may be represented as modulated by shear waves, e.g., charge density waves (spin density waves), in one, two or three directions; with the modulation period determining the displacements of atoms from their initial equilibrium positions. The periodicity of the new structure is fully commensurate with that of the initial structure: Q = nq, where Q and q are wave vectors of the commensurate and the original structures, respectively, and n is an integer. The translational symmetry is not violated in the generation of the commensurate structure. The commensurate structure can be detected by diffraction methods, e.g., through an electron diffraction observation of extra reﬂections corresponding to basic structure reﬂections for multiple distances, and by changes of other physical characteristics: electrical resistance, magnetic susceptibility, Young’s modulus, etc. The commensurate structure occurs in dichalcogenides of transition elements MX2 (M = Ta, Nb; X = Se, Te, S), in crystals of the A15 and cubic Cu2 Mg types, in the premartensitic region of temperatures in a number of compounds based on equiatomic TiNi, in Cr, etc. COMPACTION

See Pressing. COMPENSATION

See Conductivity self-compensation, Ionic conductivity compensation, Magnetic compensation.

COMPENSATION RULE, Meyer–Neldel rule (W. Meyer, H. Neldel) A relationship between the activation energy

E and the preexponential factor σ0 in the temperature dependence of the electrical conductivity σ of semiconductor:

E . (1) σ (T ) = σ0 exp − 2kB T The analysis of many experimental data obtained for semiconductors possessing current carriers with small mobilities has shown that lg σ0 = α E + β.

(2)

Here α and β are parameters characteristic of the material. Eq. (2) represents the compensation rule which has been widely investigated for polymeric semiconductors. This is explained with the help of the charge transport tunnel model (see Tunnel effect). COMPLEX ELASTIC MODULI Tensor factors in Hooke’s law written for harmonically time-varying stresses and strains in disω = sipative media (see Dissipative structures): σik ω , where σ ω and ε ω are Fourier comciklm (ω)εlm ponents of stresses and strains, respectively. The imaginary part of the complex elastic modulus, called the loss modulus, is responsible for the damping of elastic waves in a medium.

COMPLEXY

A thermodynamic equilibrium defect in a solid solution consisting of an impurity atom complex located at a group of lattice sites whose number differs from the number of complexy atoms. The concept of complexy was introduced by M.A. Krivoglaz (1970). It can be energetically advantageous to form a complexy from atoms with strongly differentiated atomic radii if this results in a partial removal of stresses and a decrease of the overall elastic energy. A complexy is less advantageous from the entropy standpoint than isolated impurity atoms, and the complexy concentration in a solid solution decreases with temperature in contrast to the behaviour of point defects. Complexy formation radically affects the temperature and concentration dependences of crystal lattice

COMPTON EFFECT

constants, diffusion coef cients, solubility of impurity atoms, diffuse scattering of X-rays, and other solution characteristics. A noticeable change in lattice parameters should be observed in alloys containing complexies, and these parameters are detected by dilatometric analysis and X-ray diffraction techniques. Complexies have been detected experimentally in a lead–gold alloy. COMPOSITE MATERIALS (fr. Lat. compositio, combination)

Materials consisting of two or more components with a distinct boundary between them, and possessing properties not found in the individual components taken separately. Anisotropic and isotropic (quasi-isotropic) composite materials are distinguished. Among the ﬁrst are reinforced composite materials including matrix and reinforcing components in the forms of ﬁbrils, wires, threadlike crystals, strips, and grids oriented in it in a predeﬁned fashion. There are metallic, polymeric and ceramic composite examples differentiated by the matrix type. Among the second are precipitationhardened materials, pseudoalloys, and randomly reinforced composites. The dispersion-hardened varieties have a matrix structure consisting of a basic material with ﬁne dispersed hardening inclusions; the pseudo-alloys can have the structure of interpenetrating skeletons, a statistical powder mixture, or a matrix structure depending on its composition and formation process; randomly reinforced materials have a matrix structure with no preferred orientation direction of ﬁbrils or inclusions. Reinforcing ﬁbrils and inclusions endow composite materials with strength, hardness, and the matrix with bonds between components, load transmission on ﬁbrils, and corrosion resistance. Properties of composite materials depend signiﬁcantly on phase boundary strength, hardening components, their size and quantity. One of the main requirements imposed on composite materials used for construction is the lack of signiﬁcant diffusion (see Diffusion) and chemical interactions of the components during the preparation and high-temperature use. By varying the structure and composition it is possible to modify the strength characteristics over a wide range, fracture toughness, electrical conductivity, thermal expansion factor, and other properties.

195

COMPOSITE MATERIALS, STRENGTH See Strength of composite materials. COMPRESSIBILITY, volume compressibility factor

Relative variation of the volume of a body under the effect of total pressure. One can distinguish the isothermal volume compressibility, κT = −(∂v/∂p)T /v = −((∂ ln(∂Φ/∂p)T )/∂p)T (Φ is thermodynamic potential) and the adiabatic volume compressibility, κS = −(∂v/∂p)S /v = −(∂v/∂p)T /v − T vα 2 /cp (where cp is the speci c heat of the body under constant pressure, α is the volume coefﬁcient of thermal expansion). The isothermal compressibility exceeds the adiabatic one for the majority of solids by not more than several percent. The compressibility has the units m2 /N = 1/Pa (typical value is ∼1/GPa). COMPRESSIBILITY MODULUS The same as Bulk modulus. COMPRESSION, UNIFORM See Uniform compression. COMPTON EFFECT (A. Compton, 1922) The scattering of an X-ray or gamma quantum off a free (or weakly bound) electron to which the photon transfers a part of its energy

and momentum. The change of the photon wavelength λ at scattering is determined by the energy and momentum conservation law and is equal to

λ = λ − λ0 (1 − cos θ), where λ is the wavelength of the scattered photon, λ0 = h/(mc) is the Compton wavelength equal to 2.426·10−12 m, θ is the angle between the directions of motion of the incident and scattered photons. The scattering intensity evaluated by quantum theory provides the angular distribution of scattered photons (mainly forward scattering) and the scattering cross-section σ which depends on the photon energy ε, with σ (ε) decreasing with ε. In the limit ε → 0 we have σ → σT = 8πr02 /3 (r0 is classical electron radius, r0 = 2.8·10−15 m). The Thomson’s scattering cross-section σT was derived by J. Thomson in the classical theory of electromagnetic wave scattering. The Compton effect can occur for scattering off other charged particles as well, but the effect is seen only for high-energy

196

COMPUTATIONAL MICROTOMOGRAPHY

photons scattering off particles with large masses. If the electron involved in the Compton scattering has a high velocity then an increase in photon energy is possible at scattering (inverse Compton effect). The Compton effect gives a strong contribution to the generation of fast electrons in gamma ray irradiated solids, and these generated electrons create radiation defects through impacts with target atoms. COMPUTATIONAL MICROTOMOGRAPHY

A method of scanning an object with a probe of penetrating radiation and, with the aid of a computer, subsequently reconstructing an image which contains details of the internal microstructure of the object in a series of thin layer cross-sections. Ordinary transmission images, being two-dimensional shadow projections of the actual three-dimensional object, do not give signiﬁcant information about its internal structure, because they display information averaged according to the thickness. In contrast to this the digitized images called tomograms (see Tomography) provide considerably sharper differentiation of areas with differing absorption coef cients, and better separation of the images of overlaying structures. To apply computational microtomography the object is transilluminated with a narrow beam of the penetrating radiation (e.g., X-rays, electrons, ultrasound, or IR) and the radiation that passes through it is recorded by corresponding detectors. By sequentially scanning the beam and/or turning the sample, a set of projection data necessary for reconstructing the tomogram is obtained. The result is a sequence of two-dimensional halftone cross-section images, and the data from these cross-sections can be used to reconstruct a threedimensional image which reﬂects the true microstructure of the object. Microtomography has been successfully used in transmission electron microscopy for the investigation of molecules, bacteriophages and membranes (with spacial resolutions of angstroms), in scanning electron microscopy, and in optical and X-ray microscopy for investigating the properties and structure of solids with dimensions of about 1 mm and resolutions of micrometers. The technique is also used in the non-destructive defectoscopy of components of solid-state quantum

electronics, providing visualization and identiﬁcation of the subsurface micro-structure and defects. See also Tomography of micro e lds. COMPUTER ALGEBRA

A process in applied mathematics and computer engineering, that uses computers for the automation of symbolic derivations. Computer algebra is designed for the execution of cumbersome (routine) analytic manipulations that cannot be readily carried out manually: multiplication (division) of polynomials, cancellation of similar terms, formation of an arbitrary algebraic expression with respect to a dependent variable, substitution of variables, integration, differentiation, etc. This approach can facilitate and improve the accuracy of subsequent numerical calculations, provide analytical relationships between various parameters, and overcome difﬁculties involved in the subtraction of nearly equal large magnitude numbers. COMPUTERS in solid state physics

Various methods for applying computers to solve problems in the ﬁeld of solid state physics. In experimental solid state physics a computer performs the following three functions: control of apparatus (e.g., the control of devices designed for molecular beam epitaxy when synthesizing superlattices); data analysis (such as deciphering various spectra); planning experiments. In an optimal situation, all these functions are coordinated, so that the computer performs quite a complicated range of research tasks. In analytical solid state physics most of the important applied problems, as well as an ever-growing share of the fundamental problems, are solved using computers. Two approaches are dominant in this ﬁeld: the numerical solution of equations, and the direct modeling of observed solid state phenomena with the help of computers (see also Computer simulation). The ﬁrst approach of solving systems of equations is not speciﬁc for solid state physics, and its efﬁciency is determined, to a great extent, by the capabilities of the computer. For single-processor computers the absolute or theoretical limit of their productivity is about 109 operations/s, but in practice the limit is lower by one or two orders of magnitude. For a relatively simple problem, such as a

COMPUTER SIMULATION

study of the initial stages of monocrystal growth from an atomic beam at a perfect monocrystal face, it is necessary to analyze a Markovian chain consisting of hundreds or (at low saturation in the vicinity of the critical point) a few thousand nonlinear differential equations. The determination of the distribution function of the atomic groupings for any given set of initial conditions requires the performance of about 108 operations/s. For a reasonably complete analysis involving the entire range of available growth conditions one needs to perform 1010 or more operations/s. The problem becomes too difﬁcult for multicomponent crystals, and indeed insoluble for single-processor computers when the ﬁnal growth stages are included in the calculation. Multiprocessor computers are also inefﬁcient in the framework of the ﬁrst approach, because extensive parallelism of the data processing is hardly achievable. In contrast, the second approach of modeling observed phenomena is quite compatible with the architecture of multiprocessor computers. The real space of the crystal can be divided into a network of conventional cells (hence the term network models) and a step-by-step analysis of changes in the states of cells and their interactions can be carried out. In the extreme case, a cell is represented by an individual atom (e.g., Ising model). The organization of this modeling system can be either linear, two-dimensional, or threedimensional. A conformity between the computational process and the processes occurring in solids is provided by means of both the programs and the apparatus. The former are universal (because the program approach allows one to model any physical process using any computer) but they do increase the duration of each step of the modeling. The latter (i.e. the apparatus part) speciﬁes the computer for each individual problem, and provides for its rapid solution. In the extreme case, the relations between the processors of the modeling system are isomorphous to the relations in the modeled solid; and the productivity increases as the number of processors increases. There exist modeling systems (so-called distributed matrix processors, “hypercube”) consisting of 105 (in order of magnitude) processors. Theoretically it is possible to produce such systems containing up to 1012 modeling processor units with a clock period

197

to 10−9 s, which permit the solution of a large part of the problems of solid state physics in real time. Further progress depends, in principle, on creating new solid and molecular modeling systems that implement the probability functions at the quantum level. In terms of the complexity of the modeling, the problems of solid state physics could be classiﬁed as follows: (i) crystallization and recrystallization in the absence of continuous defects; (ii) the same processes with the participation of dislocations and other continuous imperfect defects; (iii) electronic, thermal, and diffusion (see Diffusion) processes with changes in the location of internal boundaries (e.g., semiconductor junctions); (iv) non-structural phase transitions; (v) ﬁrstorder structural phase transitions with alteration of the lattice symmetry; (vi) second-order structural phase transitions; (vii) modeling processes on a “rigid” lattice with a quantum-mechanics analysis of elementary events; (viii) subsequent quantummechanical analysis of processes in solids with changes of lattice symmetry. At present, models of the former four types are really quite welldeveloped, and the efﬁcacy of the latter four types depends on future progress. COMPUTER SIMULATION, computer modeling

Investigation of structures and phenomena by their information simulation on computers. Direct simulation is achieved by an organization of elements of the computer and the topology of communications between them such that the properties of data-regulated processes are similar to the corresponding characteristics of the object. In this case, the maximum performance of the simulation process is achieved, but each structure and each type of phenomena need a special machine (or its complicated adjustment). Alternatively simulation is carried out by numerical treatment of mathematical equations describing the object at various boundary and initial conditions. The similarity to the object is achieved only by means of software. The hardware of simulation is universal but its efﬁciency (even at the maximum speed of the elements) is rather limited. Historically, the ﬁrst simulation was performed by analog machines for physical processes formally described by the same equations as the phenomena under

198

CONCENTRATION

study. Now there are analog machines based on various physical phenomena (transients in electric circuits, optical and acoustic waves, processes in solids and on their surface, etc.). They allow one to carry out a parallel multichannel simulation in the real-time mode of a physical process achieving an effective capacity up to and even more than 1010 –1011 operations per second. The physical structure and manufacturing techniques of such devices are relatively simple, and the energy consumption is minimal. However, besides the specialization, their shortcoming is low accuracy of calculations and instability of the simulation process. Computer simulation by numerical solution of the equations describing a physical object possesses quite opposite features. There are two approaches to computer simulation combining the advantages of digital and analog principles. The ﬁrst is based on multiprocessor computers (see Computers in solid state physics). In this case, a similarity is reached between the organization of ﬂows of the internal information exchange in a computer and mass–energy ﬂows in a modeled system. The performance of computer simulation increases by several orders; under optimal conditions, proportional to the number of processors in the system. Another approach is based on joining digital and analog processors in one device (so-called hybrid devices) in which, at each stage of simulation, the optimal distribution of data ﬂuxes between digital and analog subsystems is realized. The analog subsystem provides the maximum speed of analysis of special problems arising during simulation, and the digital one provides stability and universality of simulation, and the accuracy of the calculated data. Both approaches (digital multiprocessing and digital–analog hybrid) are based on the development of microelectronics and an increased integration of computer elements. In prospect, supermultiprocessor (up to 109 –1011 modeling cells) hybrid devices will unite the advantages of all the above-mentioned approaches to computer simulation. CONCENTRATION

The relative content of a component in a system (solution, mixture, melt). There are many different ways of expressing this: mass, moles, volume fraction, relation of individual mass or individual moles to the total. These concentrations

can be expressed as fractions, as mass or volume percentages (%), or for high dilutions as, e.g., parts per million (ppm) or parts per billion (ppb). Other ways for expressing the amount of a component and the amount of a total system are: mass concentration – the relation of the component mass to the system volume (kg/m3 , more often g/l); molar concentration (molarity) – the relation of the component quantity in moles to the system volume (mol/m3 , more often mol/l); molal concentration (molality) which is the relation of the component quantity in moles to the solvent mass (mol/kg); normal concentration (normality, n) – the number of gram-equivalents of the substance in one liter of solution; titer – the number grams of the component dissolved in 1 ml of the solution. The last two quantities are common in analytical chemistry. Furthermore, in the literature concentration is sometimes expressed as mass of the component being dissolved in 100 g of solvent, or as number of moles of the component in 1000 moles of solvent. The SI system recommends using only mass and molar concentrations. CONCENTRATION-DEPENDENT PHASE TRANSITION A phase transition characterized by the spon-

taneous onset of long-range order at T = 0 (see Long-range and short-range order) at a change in concentration of the repetative units forming

the crystal. Depending on the physical nature of the associated order parameter that arises, such a phase transition can be ferromagnetic, ferroelectric, structural, etc. Let us consider for deﬁniteness the ferromagnetic concentration-dependent phase transition in a system in which magnetic atoms replace nonmagnetic ones in a random fashion. Because the exchange interaction rapidly decreases with distance it is possible to consider as a ﬁrst approximation that only nearest neighbor magnetic atoms are interacting. At absolute zero temperature all magnetic moments coupled by exchange are oriented parallel. If the concentration x of magnetic atoms is small they form clusters isolated from each other with dimensions which do not vary with an increase of the crystal volume (ﬁnite clusters). The average magnetic moment of the whole crystal is equal to zero in this case since various clusters have oppositely directed

CONDENSED MATTER INTERFACE

199

cooling or compression. Condensation is a r storder phase transition. Vapor condensation is only

The dependence of the probability P (x) for the formation of an inﬁnite cluster on the concentration of magnetic atoms x for a simple cubic lattice.

moments. With an increase in x the characteristic size of terminal clusters increases, and at a certain critical concentration xC a cluster forms whose number of particles is proportional to the system volume, the so-called inﬁnite cluster. The magnetic moment of a crystal M(x) for x > xc differs from zero, being equal to M(x) = M(1)P (x), where M(1) is the magnetic moment of the ordered crystal, and P (x) is the probability of the formation of an inﬁnite cluster (one occupation per lattice site). Thus, at x = xc and T = 0 a phase transition from the paramagnetic state to the ferromagnetic state takes place, an effect closely related to percolation (see Percolation theory). Examples of these phase transitions in materials with interacting nearest neighbors are: semimagnetic semiconductors Cd1−x Mnx Te, Cd1−x Mnx Se, insulators SnTex Se1−x , etc. The theoretical dependence of P (x) on the concentration x of magnetic ions for a simple cubic lattice (xc = 0.31) is given in the ﬁgure. At a ﬁnite temperature T the phase transition persists, and its transition temperature Tc (x) approximately satisﬁes the condition Tc (x) = P (x)Tc (1), where Tc (1) is the temperature of the usual phase transition in an ordered crystal.

possible at subcritical conditions. Condensation to the liquid phase occurs if the temperature and pressure are above their triple point values, and it occurs directly into the solid phase if they are lower than the triple point values. The quantity of heat released at condensation is the same as that which was supplied at evaporation or sublimation, processes which are the inverse of condensation. At constant temperature condensation occurs until a vapor–condensed phase equilibrium is established which is described by the Clausius– Clapeyron equation. If the saturated vapor is a mixture of gases then this equation holds for each individual component. For the determination of condensed phases that are in equilibrium with a vapor of complex composition it is possible to make use of the complete phase diagrams. During condensation metastable phases are often formed in which the system can persist for a long time before reverting back to a more stable (at the given conditions) state (steel hardening, amorphous metal formation on cooling). Condensation throughout a volume containing vapor and on a surface are distinguished. During condensation on a cooled surface the velocity of condensing molecules has an important signiﬁcance which depends on several things: the difference between the vapor and the surface temperatures, heat exchange processes, condensation surface (solid or liquid, both continuous and dispersed), the presence of noncondensible gases, etc. The mere presence of a supersaturated vapor is not sufﬁcient for inducing condensation within the vapor volume in the absence of condensed phase particles; it is necessary to have condensation centers available (impurity particles, ions). The formation of an equilibrium nucleus of a new (condensed) phase can be unstable, and is describable by the Kelvin equation. The condensation of a vapor into a crystalline phase occurs during crystallization, epitaxy, or physical and chemical precipitation from the vapor phase. CONDENSED MATTER INTERFACE

CONDENSATION

A transition of a material from the gaseous state to a condensed (liquid or solid) one due to

A layer which separates two materials of different chemical composition that are in contact. One can distinguish geometrical and physical con-

200

CONDENSED STATE OF MATTER

densed matter interfaces. The concept of a geometrical interface is used in describing the physical properties of two bodies in contact when the layer thickness is very small compared to the bulk dimensions of these bodies so it has a negligible inﬂuence on the bulk properties. A physical condensed matter interface is a transition layer of ﬁnite thickness between bulk materials whose chemical composition differs from the chemical composition of the media in contact, and hence it can inﬂuence their properties. One can distinguish sharp and smooth interfaces. A transition layer between contacting media with a thickness the order of magnitude of an interatomic distance is called sharp, and it can be obtained by the molecular epitaxy method. A transition layer much thicker than the atomic scale is called smooth. CONDENSED STATE OF MATTER

Solid and liquid states of matter. The condensed state is characterized by high matter density in comparison with a gas, and by a rather low speed of motion of its component atoms. The regular arrangement of atoms or molecules on a three-dimensional lattice with long-range order (see Long-range and short-range order) determines the crystal structure that corresponds to an equilibrium state. There is only short-range ordering in the arrangement of atoms in a liquid. The structure of amorphous solid bodies is equivalent to that of a liquid; and from the thermodynamic point of view the amorphous state represents a supercooled liquid with a very long relaxation time for transition to the equilibrium crystal state. Macroscopic liquids and amorphous materials are isotropic. Materials intermediate between crystal and amorphous solids are polymers, liquid crystals, quasi-crystals, and the gaseous crystalline state. Polymers consist of periodic linear chains at sites where particular atom groupings are allocated. The chain molecules can be bound together in different ways. The parallel arrangement of polymeric chains deﬁnes the polymer anisotropy (see Anisotropic medium). The properties of liquid crystals are determined by the ordered orientational arrangement of their molecules which are often elongated or disk like in shape, and this results in the anisotropy of liquid crystals. There is only short-range order in the spatial arrangement of the molecule centers.

CONDENSON (fr. Lat. condensatio , densi cation, thickening)

A self-localized state of an electron in an elastically deformed medium, or a hypothetical quasiparticle in a covalent crystal in which all atomic bonds are covalent. An electron induces dipoles in neutral surrounding atoms of a medium, and then by its electric ﬁeld attracts them. As a result of small atom displacements, an increased density region is formed which represents a potential well for the electron (see Electrostriction) where it is localized. A macroscopic consideration of a condenson which takes into account a strain potential shows that if self-localized condenson states are at all possible in homopolar crystals, they will have a small radius. A macroscopic condenson can be realized in three-dimensional homopolar crystals with a “loose” crystal lattice due to weak medium anharmonicities. In onedimensional crystals a condenson can also exist in an harmonic elastic medium. A similar situation is realized, in particular, with the application of a quantizing magnetic eld to a crystal. In crystals with negative electron af nity energy (He, Ne) a reciprocal type of electron self-localization is possible with the formation of a lattice disperse region or even the appearance of a small cavity inside which the electron cloud (|Ψ |2 ) is mainly localized. CONDON APPROXIMATION See Franck–Condon principle. CONDUCTANCE, ELECTRICAL See Electrical conductance. CONDUCTANCE, HIGH-FREQUENCY See High-frequency conductance. CONDUCTION BAND An energy band of a crystal comprising elec-

tronic states with energies higher than those of ﬁlled valence bands. Weak external effects on the conduction electrons can cause a change in their average linear momentum, i.e. induce the appearance of current. To create current carriers in the conduction band of intrinsic semiconductors and insulators it is necessary to overcome an energy barrier, with

CONDUCTIVITY SELF-COMPENSATION

a minimum value called the fundamental gap (see Semiconductors). The gap ranges from about 0.1 to several electronvolts in semiconductors, and can reach about 10 eV in insulators. Typical physical mechanisms of current carrier generation are optical and thermal excitation in semiconductors, and ion collisions as well as electrical breakdown in insulators. The parameters that describe the conduction band are the same as those for the valence band: width, effective mass, presence of Van Hove singularities and their symmetry, and spin–orbital splitting (see Spin–orbit interaction). Methods for studying the conduction band include light absorption, cyclotron resonance, photoeffect, Hall effect (see Galvanomagnetic effects), etc. CONDUCTION ELECTRONS Elementary excitations (quasi-particles) of the electron Fermi liquid of metals which carry electric

charge in transport. Every quasi-particle has the same charge and spin as a free electron (exceptions are double charges (2e) in superconductors, and fractional charges in the quantum Hall effect). In the absence of external ﬁelds, the conduction electrons are characterized by the quasi-momentum p and the energy band number s. Their energy εs (p) is periodic (dispersion law) in respect to p with a period 2πb where b is a reciprocal lattice vector. A deviation of εs (p) from the quadratic isotropic dispersion law of free electrons serves as a source of numerous diverse effects which are particularly pronounced in strong magnetic ﬁelds. At a temperature T much less than the Fermi temperature T F = εF /k B (here εF is the Fermi energy, and for a typical metal, T F ∼ 105 K), the conduction electrons form a weakly-nonideal gas. A speciﬁc contribution of the electron–electron interaction to the inverse lifetime of the conduction electrons with ξ ≡| εs (p) − εF | εF is of the order of ν = (εF /)(ξ/ε F )2 . At ξ → 0, the ratio ν(ξ )/ξ → 0 which means that conduction electrons at low levels of excitation ξ εF behave as long-lived quasi-particles. This is the basis for the Landau theory of Fermi liquid describing the electronic properties of normal metals. CONDUCTIVE CHANNEL, SURFACE See Surface conductive channel.

201

CONDUCTIVITY See Electrical conductivity, Effective electrical conductivity, Electronic conductivity. Fröhlich conductivity, Hopping conductivity, Intrinsic conductivity, Ionic conductivity, Surface electrical conductivity. CONDUCTIVITY SELF-COMPENSATION A process of electrical conductivity compensation in doped semiconductors when additional

compensating defects are formed as a result of introducing free current carriers (conduction electrons, holes) into the semiconductor. The formation of the inherent compensating defect during the self-compensation may be stimulated by the introduction of impurity donor or acceptor atoms, as well as by injection of carriers through the contact or by their formation under the effect of light on an intrinsic semiconductor. Self-compensation of conductivity is effective in the case when some of the inherent defect types in semiconductors have sufﬁciently deep acceptor levels (for n-type semiconductors) or analogous donor levels (for p-type semiconductors) that the energy outlay W for thermal formation of the defects of the given type is almost completely compensated by the energy gain E in the trapping of a free carrier to the level of the forming defect. As the defect formation leads to the growth of crystal entropy S, at a sufﬁciently high temperature T and small energy difference (W − E) the minimum free energy of the crystal F = E − T S (E is the Helmholtz energy of the system) may be attained at defect concentrations ND comparable to the concentration of the carriers being introduced. Here, in the state of thermodynamic equilibrium, the actual concentration of current carriers may be signiﬁcantly lower than the concentration of impurities of donor and acceptor types with shallow levels (low ionization energies). It is not possible to obtain high conductivity over the entire series of semiconductor materials (e.g., n-Cu2 O, p-CdS, alkali-halide crystals, etc.). The kinetics of selfcompensation of conductivity is determined by the probability of the elementary act of defect formation, stimulated by the trapping of the charge carrier at a deep level during the course of defect generation. If conductivity self-compensation occurs under conditions involving the exchange of atoms between the crystal and its environment

202

CONDUCTIVITY, THERMAL

(high temperatures, pressures), then vacancies or impurity interstitial atoms may be the compensating defects. CONDUCTIVITY, THERMAL See Thermal conductivity and Thermal conductivity coef cie nt. CONDUCTIVITY, THERMALLY STIMULATED See Thermally stimulated conductivity. CONDUCTORS, electrical conductors

Materials with low speciﬁc electrical resistance (resistivity, usually below 10−6 ·m). Conductors include, for example, metals, metal alloys, semimetals (including graphite). The current carriers (charge carriers) in solid conductors are ordinarily conduction electrons. Typical for a conductor in its normal (not superconducting) state is the linear dependence of the current density on the strength of the applied electric ﬁeld (Ohm’s law). Identifying conductors as a separate class of materials can be somewhat subjective since conductivity depends on many factors, including temperature. For example, many (poor) conductors transform to a superconducting state at extremely low temperatures. CONFIGURATION INTERACTION

Interaction of multiparticle states (conﬁgurations) described by wave functions constructed

from single-particle states (see Slater determinant). The matrix elements of this interaction operator were found by J.C. Slater (1929) for orthogonal, and by P.O. Löwdin (1955) for nonorthogonal single-electron functions. The conﬁguration interaction decreases the total energy of a fermion system by the so-called correlation energy. It is necessary to take the conﬁguration interaction into account for systems with uncompensated electronic spin (atoms, ions, radicals, impurities with partially ﬁlled d- and f -shells in crystals, etc.), that is systems with unﬁlled shells. From considering a set of multiparticle conﬁgurations as the basis for solving the multielectronic Schrödinger equation, and utilizing its linearity, one arrives at the method of second quantization which is a more convenient one for treating a large number of particles. Applying the conﬁguration interaction in solids results in the narrowing of the electronic bands obtained from solutions of the Hartree– Fock equations (see Hartree–Fock method). CONFOCAL DOMAIN, focal conic domain A domain defect in a structural liquid crystal (smectic liquid crystals A, C, cholesteric liquid crystals) which has the form of a cone of rev-

olution. Because of the different orientations of molecules on the liquid crystal boundary the layers inside the confocal domain are curved with their shapes determined by the condition of maintaining an invariable width of each layer. The layers with Dupin cyclides fulﬁll this condition, as shown in Figs. 1 and 2. This results in the appearance in

Fig. 1. Conﬁguration of smectic layers in a confocal domain of a general form (left) and of a toroidal form (right).

CONFORMATIONS

203

tial spaces free of confocal domains are ﬁlled with layers of a ﬂat or spherical shape. The only discontinuities in the layer wrapping for this ﬁlling are confocal pairs. Confocal domain formation plays an important role in phase transitions and relaxation of mechanical stresses. Polarizing microscopic analysis of confocal domain structure in smectic textures has formed the basis for clarifying the onedimensional stratiﬁed structure of these media. CONFORMATIONS (fr. Lat. conformatio, shape, arrangement)

Fig. 2. Micrograph of an isolated domain in a type A smectic liquid crystal.

the confocal domain of a pair of defect lines on which the layer wrapping undergoes a discontinuity. More often one observes a confocal domain with a pair of confocal ellipses and hyperbolae situated in mutually perpendicular planes. The ellipse is located on the perimeter of the confocal domain base, and the hyperbola passes through the confocal domain vertex. In a domain with a torus conﬁguration of layers the ellipse degenerates into a circumference and the hyperbola into a line. Confocal domains with defects of a parabolic type are known as well. The confocal domain is the main element for extensively ﬁlling the layers in a liquid crystal; in particular they form confocal textures which are most commonly observed in smectics and cholesterics. At the ﬁlling, a system of adjacent confocal domains in contact with each other and of sequentially decreasing sizes is formed; the smaller domains being inserted into the gaps between the larger ones. The minimal confocal domain size is determined by the conditions of molecular orientation near the liquid crystal surface (see Boundary effects in liquid crystals). Intersti-

Different spatial conﬁgurations of a polyatomic molecule which can transform between each other without breaking valence bonds, by executing rotational displacements around single bonds, or by changing bond angles. For example, the ethane molecule C2 H6 which has a C3 symmetry axis joining the carbon atoms, changes its energy by twisting one CH3 group relative to the other in an approximately sinusoidal manner with energy maxima corresponding to D3h point group symmetry when the C–H bonds of the two CH3 groups are aligned, and energy minima corresponding to D3d symmetry when they are staggered. An example of conformations involving crystals is twinning of crystals in calcite CaCO3 wherein it is the possible to transform the unit cell from the form of a skewed prism into a direct prism, and then into a plane-reﬂected one, via a shear strain. The conformation concept is used also in a quasi-molecular deﬁnition of impurity-defect complexes and clusters, which are models of localized regions of a solid. Conformation analysis has been widely applied to cluster models for the determination of macrostructures of random semiconductor (see Disordered solids) surfaces and boundary layers. The local minima on a molecular potential energy surface correspond to stable conformations. The transition between local minima is carried out along a curve designated by K. Fukui (1970) as the path of minimum energy. Regions of multidimensional potential energy surfaces, so-called conformation maps, are useful in practice. In conformation analysis the conformer concept is introduced. It represents a set of conformations which form in the space of independent geometrical variables a continuous region including coordinates of the minimum adiabatic potential, with the region

204

CONICAL REFRACTION OF ACOUSTIC WAVES

under consideration laying below the lowest adjacent ﬁrst-order saddle point. CONICAL REFRACTION OF ACOUSTIC WAVES A special type of acoustic wave refraction on a ﬂat crystal face oriented normally to an acoustic

axis, i.e. in a direction along which a great number of quasi-transverse waves with identical velocity can propagate. An exception is the acoustic axis being coincident with a 4th or 6th order symmetry axis. Conical refraction was observed for the ﬁrst time during the propagation of acoustic waves in nickel crystals (J. de Klerk, M.J.P. Musgrave, 1955) and in dihydroammonium phosphate crystals (K.S. Aleksandrov et al., 1963). Interior and exterior conical refraction are distinguished. For the interior conical refraction the whole cone of acoustic beams corresponds to one wave normal, while for the external conical refraction the whole cone of wave normals corresponds to one beam direction. The angular opening is determined by the crystal elastic moduli and can reach tens of degrees as distinct from conical refraction of light waves. For example, it is 61◦ 30 for a calcite crystal. The special case of conical refraction in the direction of an acoustic axis located in the plane of elastic symmetry of a hexagonal crystal, when the refracted beams are distributed in a fan with a ﬂat section, was predicted by A.G. Khatkevich (1962). Under the conditions of conical refraction several effects have been observed: the reﬂection of a linearly polarized acoustic wave from a free crystal face parallel to the wave vector of an incident wave accompanied by a 90◦ rotation of its polarization plane, acoustic wave refraction on the internal surface of a twinned crystal (see Twinning of crystals), in quartz, and in a number of other ways. At ultrahigh frequencies the observation of conical refraction is complicated by acoustical activity phenomena (see Rotation of acoustic wave polarization plane). CONICAL REFRACTION OF LIGHT WAVES A special type refraction of light in optically biaxial crystals observed during propagation in the direction of any binormal optical axis (see Crystal optics). In conical refraction the thin polarized

light beam which is incident on a face of the planeparallel lamina makes up the beam in the form of

a full cone whose vertex is located at the point of the beam incidence on the face. Thus linearly polarized waves with continuously varying (in the range of 180◦ ) polarization azimuth propagate in directions of cone generators. Conical refraction was predicted by W. Hamilton (1832) and observed by H. Lloyd (1833). Internal and external conical refraction can be distinguished. Internal conical refraction occurs in light beam transmission in the binormal direction, in this case the vertex is located on the forward lamina face; on emerging from the lamina the beam makes up a hollow cylinder. External conical refraction occurs for light transmission in the biradial direction, in this case the cone vertex is located on the output lamina face. If the light beam direction does not coincide with the optical axis direction then ordinary birefringence occurs. CONOSCOPY (fr. Gr. κωνoς , a cone, and σ κoπεω, am looking, am observing)

A method of investigating optical properties of oriented anisotropic media (birefringent crystals) with the help of interference ﬁgures (so-called conoscopy ﬁgures) observed in convergent polarized light beams. In conoscopy polarized microscopes, conoscopes, and gas lasers with polarized devices are used. A conoscopy ﬁgure is obtained for light beams convergent on a birefringent crystal (uniaxial crystal or biaxial crystal) using a crossed polarizer and analyzer. The type of the ﬁgure depends on the number of optical axes of a crystal, the angles between them, the presence or absence of optical activity (see Rotation of light polarization plane), crystal lamina orientation or their combination,

Conoscopy ﬁgures obtained with light beams converging on a single crystal with crossed polarizer and analyzer: (a) for linearly polarized light, and (b) for circularly polarized light.

CONSERVATION LAWS

and polarization of light. For linearly polarized light, conoscopy ﬁgures consist of isochromates and isogyres as shown in Fig. (a). The isochromates form a family of concentric interference rings or bands, each of which corresponds to a particlar phase difference of the interfering waves; in white light the bands have a rainbow coloring. The isogyres are mutually perpendicular brushlike dark bands corresponding to directions of light transmission through the crystal in which the linear polarization is not affected. With circularly polarized light the isogyres are absent, as shown in Fig. (b). CONSERVATION LAWS of quasiparticles

Regularities whereby the values of some physical parameters of materials do not change in time. Most conservation laws existing in physics (energy, momentum, angular momentum, etc.) are applicable to solid state physics, provided the necessary conditions hold. The states of elementary excitations (quasiparticles) in crystals are characterized by a vector, similar to the linear momentum, the quasimomentum k. It is deﬁned to within an arbitrary vector of the reciprocal lattice (k and k describe physically equivalent states, if k − k = 2πb, where b is a vector of the reciprocal lattice). In the interaction of elementary excitations (the collision of quasi-particles), the law of conservation of quasi-momentum, similar to that of linear momentum, holds: k i − k i = 2πb. i

i

Here k i and k i are the quasi-momenta of quasiparticles before and after a collision. To avoid ambiguity, the quasi-momenta of all colliding quasiparticles (before and after a collision) should be “located” in the same Brillouin zone. Therefore, if the number of colliding quasi-particles is not large, the vector of the reciprocal lattice, involved in the conservation law of quasi-momentum, does not exceed one or two elementary vectors of the reciprocal lattice. Collisions with b = 0 are referred to as normal collisions (emphasizing the satisfaction of the law of linear momentum con-

205

Schematic diagram of an Umklapp process.

servation), while collisions with b = 0 are called Umklapp processes (see Fig.). A periodic crystal lattice is a space where quasi-particles exist. The law of conservation of quasi-momentum is a corollary of the symmetry (periodicity) of this space, just as the law of conservation of linear momentum reﬂects the symmetry (uniformity) of empty space. Related to the uniformity of time is the law of conservation of quasi-particle energy in a crystal ε(ki ) = ε(ki ), i

i

where ε(ki ) and ε(ki ) are energies of quasi-

particles before and after a collision, respectively. Related to the law of conservation of angular momentum is the symmetry of the stress tensor in nonpolarized media. The essential information on the interaction of quasi-particles (as well as ordinary particles) can be obtained on the basis of a conservation law analysis of their kinematics. In particular, this is how selection rules are established that forbid processes where the conservation laws do not hold. The complexity of the dispersion laws of quasi-particles and the presence of Umklapp processes make the kinematics of quasi-particle collisions very complicated: mutual particle transformations, creation and annihilation, as well as breakup and fusion of particles, are possible. Even in the case of an elastic collision of quasi-particles (e.g., electron scattering by an impurity atom in a crystal), some unusual (for particles) situations are possible, e.g., the transition from one energy band (minimum) to another band (minimum), or

206

CONSTRUCTION MATERIALS Table 1. Criteria for materials of the ﬁrst wall of a tokamak Criteria I. Radiation damages and lifetime (a) swelling (b) blistering (c) surface atomizing II. Compatibility with cooler and tritium (a) Li (b) He (c) water (d) tritium III. Mechanical and thermal properties (a) yield point (b) ultimate stress limit σT (c) creep limit (d) thermal stress parameter M IV. Processibility and welding V. Developed industry and data base VI. Cost VII. Induced radioactivity

scattering when the particles scattered in a given direction have different quasi-momenta. CONSTRUCTION MATERIALS

Materials for production of engine parts, building constructions, etc., for which shape maintenance under mechanical forces is necessary. Metals and their alloys such as steel, natural and synthetic polymers, and ceramics are used as construction materials. Composite construction materials play a special role, and for usage in aviation and astronautics a reduction in weight without sacriﬁcing strength is important. The main quality factors of these materials are strength, elastic modulus, hardness, impact strength, and temperature dependence of physico-mechanical properties. CONSTRUCTION MATERIALS FOR THERMONUCLEAR REACTORS

Materials of thermonuclear reactor (TR) elements in contact with the plasma: ﬁrst wall, aperture, and divertor. The other parts of the reactor construction are exposed mainly to neutron irradiation so the choice of materials for them is less complicated. In the advanced TR design called the tokamak the main factors which affect the ﬁrst wall are: (1) neutron ﬂux with energy up

Materials Ti, V, Mo, stainless steel C, Nb, V, Ti, stainless steel V, Ti, Al, C Ti, V, Nb, Mo, stainless steel Stainless steel, Ti, Mo, Al, C Stainless steel, Al, Ti Mo, Al, stainless steel Mo, Nb, V, Ti, stainless steel Stainless steel, Ti, Al Mo, V, Ti, stainless steel Mo, Al, Nb, V Stainless steel, Al, Ti Stainless steel, Al, Ti, C C, Al, stainless steel, Ti V, C, Ti, Al

to 14 MeV and power up to 2.5 MW/m2 , (2) heat ﬂux with power up to 0.25 MW/m2 , (3) ﬂux of neutral atoms of hydrogen isotopes D and T generated at the ion recharge, j ∼ 1020 –1021 m−2 ·s−1 . The main factors which affect the aperture and divertor receiving plates are (1) ﬂow of D+ and T+ ions and heavy impurities with energies up to 20–50 eV, j ∼ 1023 m−2 ·s−1 , (2) heat ﬂux equal to 10–20 MW/m2 . In addition in a contingency the ﬁrst wall, aperture, and divertor should be able to sustain a discharge disruption and release of all the energy accumulated in the plasma (1–2 MJ/m2 ) during a time of 20 ms. For uncontrollable modes of TR operation the aperture and divertor can erode because of the development of unipolar arcs, i.e. electrical discharges between the plasma and plasma trap chamber. For design and economy reasons the ﬁrst wall cannot be changed, and should operate in an industrial reactor for ∼30 years. Aperture and divertor receiving plates are changeable. Table 1 cites main criteria for choice of materials for the ﬁrst wall of a tokamak listed according to their priority. The thermal stress parameter M M=

2σT k(1 − ν) , αE

CONTACT ANGLE

where k is the thermal conductivity, α is the thermal expansion, E is Young’s modulus, and ν is the Poisson ratio, characterizes the thermal stress from the temperature gradient: the greater the M value the greater is the allowable wall thickness. The tokamak operates in the pulsed mode, and the international reactor INTOR pulse lasts 200 s with a 20 s pause between. Thermal load cycling promotes the aging of materials. The most important features for the material choice for the aperture and divertor receiving plates are thermal and chemical properties, and surface erosion. For a hybrid reactor combining a thermonuclear and ﬁssion reactor which uses thermonuclear neutrons, construction materials will have less plasma applied loads because the high power of thermonuclear energy is not required, but the materials are subjected to radiation exposures typical of those from atomic ﬁssion reactors. CONSTRUCTION MATERIAL STRENGTH

The strength of construction materials or their models having design shapes and geometrical sizes typical of actual construction elements. In contrast to the material strength which is evaluated experimentally by testing relatively small material samples on devices of simpliﬁed shape, the constructional strength is evaluated by testing material samples with geometrical shapes and sizes that are typical of the majority of actual parts of engines or other devices. Values of constructional strength are much lower than those of material strength which is generally obtained for simpliﬁed laboratory samples. This difference arises mainly from the design shapes which often involve sharp transitions from one section size to another, the presence of holes which induce some stress concentration, and other factors. In addition, the surface quality of actual samples can differ considerably from the surface of laboratory ones because the handling technology of actual device production, as a rule, differs from the technology used for preparing simpliﬁed laboratory samples. The strength indices of actual samples are strongly inﬂuenced by their production technology, especially by welding which causes inhomogeneities in the material, and also the tangent stress due to so-called welding stresses.

207

Constructional strength is appreciably degraded by the decline of performance factors arising from exposure to repeatedly changing loads. There are always a number of factors under actual working conditions which cause the concentration of stress to be the main origin of the appearance of fatigue cracks on exposure to repeatedly changing stresses. CONSTRUCTION PLASTICS

Plastics (see Polymeric materials) designed for the production of parts and components capable of keeping their shape during exposure to mechanical loads. Polyoleﬁnes, polyformaldehydes, polyamides, ﬂuoroplasts, polyarylates, etc. are used in various industries as constructional plastics. The main processing methods for converting these plastics into components are pressure die casting, hydroextrusion, and pressing. In most cases constructional plastics are multicomponent systems: antioxidants, lighting stabilizing agents, plasticizing agents, oilers, bulking agents, etc., which are loaded as additional binders that impart speciﬁc properties (e.g., ber glass, carbon, boron nitride, ﬁre-retardant additives, etc.). CONTACT ANGLE

Angle between surfaces of a ﬂuid and a solid body (or another ﬂuid) in contact. The contact angle θ is counted from the ﬂuid. The equilibrium contact angle is referred to as the edge angle and is denoted by θ0 . During contact formation the angle varies from θ = π up to θ ≈ θ0 during 0.02–0.03 s. On rough solid surfaces the contact angle usually decreases, so that for θ < π/2, cos θ = γ cos θ0 , where γ is the surface roughness coefﬁcient. The contact angles for ﬂuid inﬂow on a substrate θin , and for outﬂow θex , differ from θ0 . This is caused by the roughness and heterogeneity of the actual surface. For substrate backings with a high surface energy the property of “autophobia” is possible in contact with polar ﬂuids: the ﬂuids on the substrate generate adsorption ﬁlms on which they form a contact angle θ > 0. It is known that θin > θ0 > θex , and this effect is referred to as wetting hysteresis. With increasing

208

CONTACT CORROSION

temperature θin → θ0 and θex → θ0 , so the hysteresis decreases (see Wetting). CONTACT CORROSION, galvanic corrosion A type of electrochemical local corrosion re-

sulting from the contact of two or more metallic materials with different initial corrosion potentials, situated in a conductive corrosion environment. The contact corrosion intensity is determined by a polarization cathode and anode resistance, the ratio of their dimensions, and decreases with increased distance from the contact point. The metal quantity being dissolved because of contact corrosion is equivalent to the current. Methods for protecting against contact corrosion consist of sensible equipment designing, eliminating or isolating contacts of metals having much different corrosion potentials, using protectors, etc. CONTACT POTENTIAL DIFFERENCE

Difference of electric potentials between surfaces of conductors brought into contact at thermodynamic equilibrium. It is deﬁned by the difference in the work functions of the media in contact divided by the electron charge. The contact potential difference arises from the requirement of electrochemical potential equality for media in contact; it is established because of electron exchange between the conductors. Thus the surfaces of both media become charged: negative for the conductor with the greater work function, and positive for the other. The width of the boundary (contact) layer in which the electric ﬁeld differs from zero is deﬁned by the shielding distance in the conductor, with values 10−10 –10−9 m for metals and up to 10−6 m for semiconductors. The potential difference can reach several volts, and depends on the physico-chemical condition of the boundary region. In multiple layer heterophase structures representing a chain of conductor contacts the overall potential difference does not depend on the intermediate links, but equals the potential difference of the extreme outer conductors. This potential difference is important for the formation of electrovacuum devices and solid contact structures: semiconductor junctions, heterogeneous structures, metal–semiconductor junctions, etc.

CONTACT PROBLEM OF ELASTICITY THEORY Determination of the strain and stress distrib-

ution in a system of solid bodies having a general contact surface. For the case of two elastic bodies in three-dimensional space this problem was set up and solved ﬁrst by H. Hertz (1882) by considering that the contact area consists of small, strain-free surfaces around the contact point referred to as second-order surfaces. With the help of an electrostatic analogy he determined the pressure function at the contact point, and derived explicit formulae relating the magnitude of the impression h, the impressing force F , and the main radii of curvature of strain-free surfaces at the contact point, from which a relationship of the type h = const · F 2/3 followed. Among contact problems of the theory of elasticity are stamp problems in which one of contacting bodies is an elastic halfplane, and the other is an perfectly rigid body impressed into the halfplane by ﬁxed forces. In the simplest case of a ﬂat die uniformly pressed onto the boundary of a half-plane on the segment (−a, a) of the Ox axis the contact pressure distribution P (x) is determined by the formula P (x) = F /[π(a 2 − x 2 )1/2 ] where F is the pressing force. One approach to solving such a problem involves reducing it to a boundary value problem of the theory of analytical functions. CONTACT STRESSES, mechanical

Stresses which appear at mechanically interacting solid deformable bodies, or around them (e.g., at the compression of bodies in contact). Knowledge of contact stresses is important for the strength calculation of bearings, gear and worm transmissions, ball and cylinder compactors, colliding bodies, etc. The contact surface size is often small in comparison with the body dimensions, with the contact stresses rapidly decreasing with distance from the initial contact point. The stress distribution at the contact area and in its neighborhood is nonuniform, and the peak shearing stresses which characterize the strength of compressed bodies can appear at a particular distance from the contact point. In Fig., the upper part shows two spheres in contact, subject to the compression force P , with A indicating the point of peak stress. The lower part shows how the stress p in the interface decreases with the radial distance r

CONTINUUM MECHANICS

209

a Euclidean space, however, any part of such a sphere is homomorphic to a certain region of Rn . Lie groups are among the most important transformation groups used in physics. For example, various conservation laws are related to such groups. The Lie groups most often found in physics are the orthogonal groups O(n) and the unitary groups U (n) of real- and complex-valued n × n matrices, which preserve their scalar product in the real, Rn , and complex, Cn , Euclidean spaces, respectively. Their subgroups consisting of matrices with a unit determinant (det = +1) are called special orthogonal groups and special unitary groups, denoted by SO(n) and SU(n), respectively. Spherical harmonics transform by SO(n), and spinors (S = 1/2) by SU(2). CONTINUUM INTEGRAL See Path integral. CONTINUUM MECHANICS, mechanics of continua

Upper part: two spheres in contact subject to the compression force P , with the point of peak stress designated by A. The region of contact has the radius a. Lower part: the stress p variation with the radial distance r from its peak value p0 in the center.

from its peak value p0 in the center of the contact area. See also Contact problem of elasticity theory. CONTINUOUS SYMMETRY TRANSFORMATION GROUPS, Lie groups (S. Lie)

Transformation groups with continuous symmetry. Inﬁnite groups in which a ﬁnite number of parameters, n, corresponds to each element of the group. Here, the group operations (i.e. mappings (g, h) → gh and g → g −1 for elements g and h of a group G) must be continuous and inﬁnitely differentiable functions in the parameter space. A number n is called the group dimensionality. In general, the n-dimensional Lie group is a topological space (differentiable manifold), the neighborhood of each of its points being homomorphic to a certain region in Euclidean space Rn . For example, an n-dimensional sphere Sn is not

Branch of mechanics devoted to describing the properties and movements of matter (solids, liquids, gases, plasma, etc.) in the continuum approximation. This approximation involves long wave length vibrations (λ lattice constant) with small propagation constants k = 2π/λ. The mechanics of continua may be divided into the mechanics of deformable solids (including elasticity theory, plasticity theory, theory of failure, etc.), hydrodynamics, gas dynamics, etc. The continuum approximation applies to any dynamic system that consists of a large number of particles that may be considered as a homogeneous medium. This description is predicated on introducing physically inﬁnitesimal volumes, whose size (l mic ) far exceeds characteristic distances between particles (l part ). Averaging microscopic mechanical characteristics of the system (forces, coordinates, momenta of particles, energy, etc.) yields macroscopic quantities (density, velocity ﬁeld) that have a continuous distribution in space. The equations of motion of particles undergo a similar averaging; to obtain closed form equations for the above macroscopic quantities. To accomplish this it is necessary, as a rule, to perform a certain “uncoupling” of cross-terms of dynamic equations. The latter procedure imposes a limitation on l mic ,

210

CONTINUUM MECHANICS

i.e. l mic l mac , where l mac is the characteristic length of variations of averaged macroscopic quantities. One can obtain in this manner, e.g., hydrodynamic equations from quantum equations of motion of the density matrix, or equations of elasticity theory from classical equations of motion of crystal ions. Thus the validity criterion for the present description of a dynamical system of a large number of particles is of a self-consistent nature, and is stated in the form of an inequality l part l mic l mac . This criterion corresponds to sufﬁciently homogeneous systems (gases, liquids). In the case of inhomogeneous systems that contain many (macroscopic) structural elements this description may prove to be too detailed, and it may be necessary to perform a second averaging of macroscopic equations of motion over volumes of a larger characteristic size l that satisﬁes the . Here, l inequality l str l lm str is the characteristic size of structural elements or the mean is the characteristic distance between them, and lm length of variations of doubly averaged quantities. Typical examples are the averaged description of the motion of multiphase media with a heavy mixing of phases (i.e., attenuation of sound in solids with many pores, or the elastic properties of a composite material), plastic ﬂow of solids under conditions of a high density of dislocations and dispersed particles, and the possible propagation of a main crack in a material with a number of microcracks and cavities in the zone of failure. Two equivalent methods are used for describing the motion of macroscopic particles of continuous media. The Lagrange method involves tracking the location of a particle r = r(a, t) at every instant of time t ; vector a speciﬁes the particle, and is usually taken to be the particle location at the initial instant of time t0 . The Euler method involves tracking the velocities, accelerations, etc. of various particles that pass through a certain point r of the space. Ordinarily the Eulerian description is used when the mechanical state of the medium is characterized by ﬁelds of various types: displacement ﬁeld u(r, t), velocity ﬁeld v(r, t), density ﬁeld ρ(r, t), etc. The ﬁelds usually satisfy second-order partial differential equations (Navier–Stokes equations of hydrodynamics, equations of elasticity theory, etc.). Along with u and v, these equations involve the force characteristics of the medium, described most often by

the ﬁeld of the stress tensor σik (r, t). Evaluating the system of equations of the mechanics of continua requires specifying the constitutive relations (rheological equations) that establish a link between σik and u, v. In the case of a solid under smooth and rather small strain, this link may be considered linear and local (i.e. σik (r, t) depending on the values of u, v, taken at the same point r and at the same instant of time t ). More complicated relationships between σik and u, v are also possible (linear, nonlocal, with allowance for the history of deformation of the medium), represented by complicated functions σik = fik (u, v) or by functionals σik = &{u(r, t), v(r, t)}. For instance, we have for a linear nonlocal medium Alm σik (r, t) = ik (r, t; r , t )ulm (r , t ) dr dt . Equations of continuum mechanics in the linear local approximation often proceed from general considerations (law of conservation of particle number, symmetry conditions, etc.). They contain a number of unknown coefﬁcients (elastic moduli, coefﬁcient of viscosity, etc.) that should be determined experimentally or calculated from a microscopic theory. The above procedure for obtaining macroscopic equations from microscopic ones involves not only purely spatial averaging, but also statistical averaging (for quantum dynamic systems both kinds of averaging are performed simultaneously through the density matrix). Statistical averaging may fail to produce closed mechanical equations, since the continuum equations may contain thermodynamic and chemical quantities (temperature, concentration, chemical potentials, etc.) along with parameters characterizing internal degrees of freedom of microparticles or other subsystems of the body (electric, magnetic, and others). In this case, the mechanical problem should be solved together with the thermal, chemical, etc. ones by adding equations of thermal conductivity, diffusion, etc. to continuum mechanics equations. Typical examples are diffusive-viscous creep of polycrystals (see Diffusion mechanism of crystal creep), dynamics of ferroelectrics and ferromagnets, and propagation of shock waves in crystals. Besides that, empirical or calculated relationships may be available, which describe the

COOLING DUCT

dependence of mechanical parameters (e.g., elastic constants) on temperature, concentration, magnetization, etc. The most consistent description of related mechanical, thermal, electrical, and magnetic processes can be made within the framework of the thermodynamics of irreversible processes, which includes much of continuum mechanics as a special case. In certain situations, however, one can conﬁne oneself to the solution of a purely mechanical problem. For instance, in a static state during a very slow deformation of a solid, the temperature has time to equilibrate and the deformation process is described by equations of elasticity theory with isothermal elasticity moduli. Also, under very rapid deformation (e.g., propagation of high frequency sound), heat transport between neighboring parts of a body does not take place, and the process is described by the same equations, but with adiabatic elastic moduli. CONTINUUM THEORY OF DEFECTS Theory of defects in a broad sense based on

the continuum approximation in analysis. From a more specialized viewpoint the continuum approach to defects is founded on the assumption that they ﬁll the physical space of the crystal. The subjects of this analysis are usually dislocations, disclinations, dispyrations, and planar defects, although the methodology can be extended to other problems which are not closely related to the presence of defects: e.g., this theory is used for the calculating thermal stresses, electrostrictive or magnetostrictive mechanical effects (see Electrostriction, Magnetostriction), elasto-plastic ﬁelds generated by phase transitions or twinning of crystals, etc. This continuum theory is constructed on rather general physico-mechanical principles. It includes the determination of the tensor of densities of defects, the balance conditions for these densities, and the continuity condition (existence of solutions). In this theory the connection between defect motion and the plastic ﬁelds generated by this motion (see Plastic deformation) is analyzed. The forces acting in this process and other factors are evaluated. The system of equations in the continuum theory involves a fundamental relation that connects the mobility of defects and the forces acting on them. This fundamental equation is considered to be known because it cannot be

211

derived, apparently, within the framework of the continuum approximation. CONTRACTION, TRANSVERSE

See Transverse contraction. CONVOLUTION OF LINE SHAPE

See Line shape convolution. COOLING AGENT, refrigerant

A material (working medium) used to cool a substance (cooling agent) or maintain it at a low temperature (cryo-reservoir). The most widely used refrigerants are liquids and gases with low condensation and crystallization temperatures (3 He, 4 He, H2 , Ne, N2 , CO2 /acetone, etc.), paramagnetic salts (magnesium cerium nitrate Ce3 Mg3 (NO3 )12 ·24H2 O, ferric chromium alum and ferric aluminum alum), van Vleck paramagnets (PrNi5 , PrPt5 , PrTl5 , PtCu6 , etc.), metals with paramagnetic nuclei (Cu, Ag, In, etc.). COOLING DUCT

A heat exchanging device to provide the thermal connection of an object being cooled with a cooling agent (refrigerant), or with a cryostat (low-temperature reservoir). In the simplest case a cooling duct is a rod (tube, stripe, etc.) of a material with good thermal conductivity, which provides a reliable thermal connection with the parts of an installation containing the object being cooled, as well as the cooling agent, or the low temperature reservoir. Often (especially at low temperatures) the cooling duct is in the form of a large number of thin wires (usually made of copper) which improves the heat transfer efﬁciency by increasing the contact area. To arrange for the adjustment of the temperature the cooling duct can be provided with a heater, and when it is necessary to rapidly change the thermal connection then heat switches are used. The associated properties of a thermal switch and a cooling duct are combined in a thermosiphon, which is an hermetically sealed tube ﬁlled with a gas under pressure, providing for its liquefaction in the desired temperature range.

212

COOPERATIVE LUMINESCENCE

Cooperative luminescence.

COOPERATIVE LUMINESCENCE Luminescence caused by radiative transitions

from excited states in crystals that result from the delocalization of energy from individual excited states (e.g., photoexcited states of impurity centers); it is a special case of anti-Stokes luminescence. Cooperative luminescence violates the Stokes’ rule and Vavilov law. The phenomenon was discovered by C.A. Parker (1962) and F. Muel (1962) in dye solutions. In the solid state it was observed by P.P. Feoﬁlov, V.V. Ovsyankin (1966) and separately by F. Auzele (1966) in crystals activated with rare-earth ions, and in broad-band semiconductors with an adsorbed dye. An example of the mechanism of cooperative luminescence is the absorption of light by local crystal centers (transitions 1 → 2 and 1 → 2 ), the addition of photoexcitation energy to induce the transition from one of these excited states to the 3 level, followed by the subsequent radiative transition 3 → 1 (Fig. (a)). This luminescence process can also occur through excitation energy transport from two local centers (2 and 2 levels) to a third (level 2 ), with the subsequent radiative deexcitation of the latter (2 → 1 ) (Fig. (b)). COOPER EFFECT (L. Cooper, 1956)

Instability of the ground state of a fermion system with respect to the spontaneous formation of bound pairs of fermions with antiparallel momenta and spins (see Cooper pairs), provided that an arbitrarily weak attraction V0 < 0 exists between these particles in a narrow energy band near the Fermi surface. The binding energy of a selected pair of fermions (lowering of its energy with respect to the Fermi level, EF ) is equal to

E = ω0 e−2/g , where g = N(EF )V0 is the dimensionless coupling constant, N(EF ) is the density of states at the Fermi surface, and ω0 EF . In momentum space the Cooper effect is similar to the quantum-mechanical formation of a bound state that develops when a particle of mass m moves in a two-dimensional rectangular potential well of depth U0 and width a. Within the limit of weak coupling (shallow and narrow well) the energy of the lowest level depends exponentially on the interaction constant: E0 ∝ U0 e−1/g0 , where g0 ∝ U0 a 2 m/2 . While treating the problem initially and selecting an isolated pair of fermions (i.e. electrons) from the Fermi sea, L. Cooper ignored the principle of particle identity, but took into account the Pauli principle. A more systematic self-consistent treatment of the problem was provided by J. Bardeen, L. Cooper and J. Schrieffer (1957) (see Bardeen–Cooper–Schrieffer theory). COOPER PAIR, KINETIC DECOUPLING See Kinetic decoupling of Cooper pairs. COOPER PAIRS

Correlated bound states of fermion pairs (electrons, sometimes holes) with opposite quasi-momenta and antiparallel (singlet) or parallel (triplet) spins, that form due to an attractive interaction (see Cooper effect). Such an attraction in metals (semimetals, doped semiconductors etc.) between conduction electrons (holes) near the Fermi surface at low temperatures can be produced by the exchange of virtual phonons. For a strong enough electron–phonon interaction the attraction may override the screened Coulomb repulsion. The Cooper pairs formed by this attraction have the binding energy 2Δ EF (Δ is the energy gap, EF is the Fermi level), and are characterized by a correlation radius larger than the average electron-to-electron distance r = 10−9 m. This is the so-called coherence length ξ = 10−8 m, so that the wave functions of Cooper pairs strongly overlap. As a result a coherent condensate of Cooper pairs forms within the volume of the crystal (see Bose condensate) that is described by a complex wave function ψ = |ψ|eiθ (the order parameter) with a phase θ that is, generally, coordinate dependent. Since the spin of a Cooper pair

COORDINATION SPHERE

is an integer (0 or 1) it is a Boson particle, and a Bose–Einstein condensation called a Cooper pair condensate can form in which all of the pairs are in the same quantum-mechanical ground state. However, Cooper pairs have been called “bad” bosons + + a−p,−σ and annihisince their creation Bp+ = apσ lation Bp = a−p,−σ apσ operators are more com+ plicated than the usual creation apσ (annihilation apσ ) operators of a fermion with momentum p and spin s = ±1/2 (see Second quantization). Cooper pairs have the more complex commmutator relations Bp Bp+ − Bp+ Bp = (1 − npσ − n−p,−σ )δpp , instead of the usual Bose operator commutation rules. Here δpp is the Kronecker symbol and + apσ is the number operator, which npσ = apσ is 1 for an occupied state and 0 for an unoccupied one. The Cooper pair condensate state is separated by a gap of 2Δ from excited states (excitations above and below the Fermi surface), the latter having a continuous spectrum εp = ±(Δ2 + vF2 (pF − p)2 )1/2 that satisﬁes the Landau super uidity criterion (vF and pF are the Fermi velocity and Fermi momentum, respectively). Thus, the formation of Cooper pairs in a charged electron Fermi liquid (or Fermi gas) in metals results in superconductivity, while in a neutral Fermi system (3 He, neutron matter) a process involving rotons results in the related phenomenon of super uidity (see Super uid phases of 3 He). COORDINATION COMPOUNDS

These are compounds of complex composition in which a central atom or ion (complexing agent) has molecules and ions called ligands bound to it by donor–acceptor bonds (see Donor–acceptor pairs). The central metal atom or ion is generally a transition metal with electron-acceptor properties. Ligands representing electron donors can be neutral molecules (H2 O, NH3 , CO, etc.) or − anions (C2 O2− 4 , CN , etc.). The central atom together with its ligands form the “complex” or inner coordination sphere of complex compounds, and examples are [Fe(CN)6 ]3− , [Co(NH3 )6 ]3+ and [Pt(NH3 )2 Cl2 ]. The inner sphere is usually enclosed in square brackets. The complex can be neutral or charged, in the latter case it is a cation

213

(+) or anion (−), and counterions (monatomic or complex) comprise the outer coordination sphere. To separate the complex ion from its component + ions such as SO2− 4 or NH4 one can assume that the reaction of complex formation from the central atom (ion) and ligands can occur under normal chemical conditions, and that the central ion is capable of existing independently in solution in a solvated form. This limitation is of a conditional character since there is no essential difference be− tween such ions and, for example, PF− 6 and VF6 in their chemical bond nature, and the majority of their physico-chemical characteristics. Each ligand is attached to the central atom through one, two, or several atoms occupying, respectively, one (monodentate ligand), two (bidentate ligand) or several (polydentate ligand) coordination sites. The total number of coordination sites in a complex is its coordination number, and it is determined by the central atom oxidation state and by the nature of the ligand. Complexes with coordination number six and octahedral symmetry are the most widespread ([PtCl6 ]2− , [Ru(NH3 )6 ]2+ ); others are commonly four-fold coordinated with square planar ([PtCl4 ]2− ) or tetrahedral ([CoCl4 ]2− ) symmetry. Coordination polyhedra can be distorted through ligand inequivalence, electronic effects (see Jahn–Teller effect) or crystal lattice inﬂuences. COORDINATION SPHERE

A sphere centered at a particular atomic site with surrounding atoms of the crystal located on its surface. Coordination spheres are numbered in the ascending order of their radii: the ﬁrst (closest), then the second, and so on. The ﬁrst sphere contains the z nearest neighbors of the given atom, where the coordination number z is is a measure of the packing density of the atoms; the most loosely packed semiconductor structure is the diamond type (Si, Ge) with z = 4, in NaCl type ionic crystals z = 6, in BCC metals and those with the ﬂuorite structure (ceramics) z = 8, in FCC and HCP metals z = 12. In ideal crystals the coordination sphere radii coincide with peak positions of the radial distribution function (RDF), with the number of atoms in the nth sphere proportional to 4πrn2 Sn , where Sn is the space under the nth RDF surface. Using this correspondence, the coordination sphere concept can be extended to liquids and

214

COPPER

amorphous solids (see Amorphous state), understanding as the nth coordination sphere the spherical layer with atom positions within the range rn of radius values rn corresponding to the magnitude of nth RDF peak, and considering the number of atoms in the nth sphere as 4πrn2 Sn ρ, where ρ is the average atom density. For an amorphous solid, with increasing r the RDF peaks rapidly broaden and become ﬂattened, so the coordination sphere concept is used only for small n (usually n = 1–3). Thus, in virtue of the statistical nature of the RDF the number of atoms in the sphere (the coordination number) can be nonintegral. The coordination sphere concept is useful in the analysis of structures with short-range order (see Long-range and short-range order), for self-ordered alloys, for the approximate construction of a crystal potential for band structure calculations, and so on. COPPER (Lat. cuprum ), Cu

Chemical element of Group IB of the periodic table with atomic number 29 and atomic weight 63.546. Stable isotopes 63 Cu (69.1%) and 65 Cu (30.9%). Nine radioactive isotopes are known. Outer shell electronic conﬁguration 3d 10 4s 1 . Successive ionization energies (eV): 7.72, 20.29, 36.83. Atomic radius is 0.127 nm. Ionic radii are (nm): Cu+ 0.096, Cu2+ 0.072. Covalent radius 0.117 nm. Oxidation states +1, +2, more rarely +3. Electronegativity is 1.75. Copper is a red-tinted metal of face-centered ¯ (O 5 ); a = cubic structure, space group F m3m h 0.361479 nm. Density is 8.932 g/cm3 ; Tmelting = 1356 K, Tboiling = 2843 K, heat of melting 13.0 kJ/mole, heat of sublimation 340 kJ/mole, heat of evaporation 307 kJ/mole (under standard conditions). Speciﬁc heat is 390 J·kg−1 ·K−1 at 298 K. Debye temperature is 339 K; linear thermal expansion coefﬁcient 16.8·10−8 K−1 . Coefﬁcient of thermal conductivity is 385–402 W·m−1 ·K−1 (at 273 K) and 5 W·m−1 ·K−1 (at 20 K). Adiabatic elastic moduli of crystal: c11 = 168.8, c12 = 121.8, c44 = 75.5 GPa at 298 K. Young’s modulus is 110–145 GPa, shear modulus is 42–55 GPa, Poisson ratio is ≈0.33. Rupture strength is ≈230 MPa, relative elongation 60%. Brinell hardness is 35 HB (at 293 K). Coefﬁcient of selfdiffusion is 9.1·10−14 m2 /s (at 1233 K). Lowtemperature linear electronic heat capacity coefﬁcient 0.687–0.695 mJ·mole−1 ·K−2 . Electric

resistivity is 15.5 n·m. Electric resistance temperature coefﬁcient is 440·10−5 K−1 (at 273– 373 K). Hall constant is −5.2·10−11 m3 /C. Absolute thermal electromotive force coefﬁcient +1.7·10−6 V/K. Reﬂection factor for 5 μm optical wave is 98.9%. Work function of a copper polycrystal is 4.4 eV. Copper is diamagnetic with magnetic susceptibility (5.4–10)·10−6 CGS units. Ion plasma frequency is 7.655 THz. About 50% of copper produced is used in the electrical power industry, and over 30% is used for copper alloys. It is widely used for chemical equipment. COPPER ALLOYS Copper forms the following systems with other elements: (a) inﬁnite solubility in solid and liquid

states: with Ni, Rh, Pt, Pd, Mn, Au; (b) inﬁnite solubility in liquid and limited solubility in solid state: with Li, B, Ag and Bi; (c) peritectic type of interaction (see Peritectic alloys): with Ir, Nb, Co, Fe; (d) limited solubility in liquid and solid phases: with Pb, Tl, Cr, V); (e) intermediate compounds with many elements (for dissimilar electrochemical properties Cu forms chemical compounds; for the same properties, an electron compound is formed). Cu dissolves up to 31.9 Zn, 20 Li, 16.6 Be, 16.4 Ga, 15.8 Al, 12 Ge, 11.15 Si, 10 In, 8 Ir, 8 Ti, 8 Sb, 7.7 Sn, 7 Mg, 6.85 As, 4.5 Fe, 3.4 P, 2.1 Cd (molar content, %). Some copper alloys have special names: bronzes (with Al, Sn and some others), brasses (with Zn), German silver (with Ni). On addition of Zn, Sn or Al to Cu, α-solid solutions appear ﬁrst; then, as the concentration increases, β-, γ -, δ-phases appear, and so on. All industrial brasses and bronzes are of two types differing in structure and properties: single-phase α-alloys (plastic, easily deformable, strength and hardness slightly exceeding those of copper) and two-phase alloys (α-solid solution + another phase). The latter exhibit higher strength and hardness but lower plasticity. Of practical use are brasses that contain up to 43% Zn, tin bronzes with up to 22% Sn, aluminum bronzes that contain up to 11% Al. Tin bronzes exhibit enhanced strength, hardness, corrosion resistance (α-bronzes that contain up to 7– 8% Sn). Aluminum bronzes are stronger and more plastic, corrosion- and wear-resistant; two-phase alloys are commonly used (≈ 10% Al). Quenching and tempering (because of phase transitions

CORRELATION ENERGY

in the solid state) may change their properties essentially. Silicon bronzes exhibit less speciﬁc weight and high mechanical properties. If silicon content is 2–5%, they are mostly single phase and often used with Mn, Fe, Zn additions. Beryllium bronze (2–3% Be) exhibits high elasticity, corrosion resistance. In cadmium bronze Cd improves the strength of Cu. Lead bronze separates into layers already in the liquid phase; at Pb content of 20–30%, it is used as a bearing alloy. Cu forms the following compounds with Ni: copper– nickel (32% Ni), constantan (40–45% Ni) that exhibits high electrical resistance, bullet German silver (20% Ni). Single phase alloys with Mn possess enhanced electrical resistance: manganin (12% Mn + (2–4)% Ni) and double manganin (20% Mn + 5% Al) with electrical resistance twice that of manganin. CORBINO DISK (O.M. Corbino, 1911)

A metal or semiconductor disk with a hole in the center, with a contact located on the inner wall of the hole, and another at the periphery. It is used for investigating galvanomagnetic effects. The plane of the disk is normal to an external magnetic ﬁeld B. When electric current ﬂows between the contacts, due to the sample axial symmetry the electric ﬁeld has only a radial component and the Hall ﬁeld is absent. As a result, there is no (partial) compensation for the curvature of charge carrier paths in the magnetic ﬁeld by the Hall ﬁeld, and the relative resistance R/R in the magnetic ﬁeld appears to be much greater than the magnetoresistance value ρ/ρ0 (ρ0 is the resistance with the ﬁeld absent, and ρ is the change brought about by the ﬁeld) measured in a long (thread-like) sample. In n-InSb at 300 K in a ﬁeld B = 1 T,

R/R = 17.7, and ρ/ρ0 = 0.48. These values are connected by the relationship

R

ρ (μH B/c)2 = + R0 ρ0 1 + ( ρ/ρ0 ) (μH is the Hall mobility of charge carriers) from which it follows that when B increases the ratio

R/R does not tend to saturation. Therefore, the Corbino disk is utilized in devices for strong magnetic ﬁeld measurement (see Magnetometry).

215

CORRELATION in alloys

The interconnections in the equilibrium distribution of alloy component atoms on crystal lattice sites. They depend on the differences in the interaction energies of different atoms since each atom tends to surround itself by atoms of another type in ordered alloys, or by the same atoms in dissociating alloys (see Alloy ordering, Alloy decomposition). Quantitative measures of this correlation are correlation parameters, or short-range order parameters. The latter characterize mainly the extent of the formation of pairs of dissimilar atoms, or pairs of identical ones. CORRELATION ENERGY

The difference between the ground state energy of an interacting particle system and the minimum energy of the system determined by a selfconsistent eld method. The correlation energy concept is most often used for the description of an electron gas. For the self-consistent Hartree–Fock method the correlation energy is the true energy minus the kinetic, electrostatic and exchange energies. In this case the correlation energy is related to the decrease in energy due to the vanishing of the probability density for the presence of two electrons at the same point because of the singularity of the Coulomb interaction. A rigorous calculation of the correlation energy always represents a complicated problem, especially when dealing with a crystal or a polyatomic molecule. In such cases the wave function is represented by a superposition of antisymmetrized products of one-particle states (in Hartree–Fock theory only one such term is retained), see Con guration interaction, or the wave function is formed on the basis of two-, three-, and so on molecular orbitals (e.g., geminals). The correlation energy of a homogeneous electron gas is the best studied. Here the energy, according to Hartree–Fock theory, corresponds to the ﬁrst order of the perturbation theory of the interelectronic interaction, and the correlation energy is the sum of the remaining terms of a series, each term of which diverges. Several ways are known for summing these series that result in the expansion of the one electron correlation energy 22 εcorr = 2(1 − ln 2) ln rs − 0.096 + Ars ln rs me4 + Brs + · · · ,

216

CORRELATION ENERGY OF A CENTER

where rs = [3n/(4π)]1/3 is the average distance between electrons in Bohr radii [2 /(me2 )], and n is the number of electrons per unit volume. This expansion in powers of rs cannot be rigorously justiﬁed for real valence electron densities for which 1.5 < rs < 6. Nevertheless, the known results for the correlation energy are in good agreement with those obtained with the aid of the variational principle, that are not dependent on the smallness of rs . The correlation energy of inhomogeneous systems is more often calculated within the framework of density functional theory (see Density functional theory) using the approximation of local homogeneity. This gives Ecorr = εcorr n(r) n(r) d3 r. The exchange interaction energy is not always separated from the correlation energy, and then one speaks about an exchange-correlation energy. CORRELATION ENERGY OF A CENTER

The difference U between the energies E1 and E2 in the sequential trapping of the ﬁrst (1) and the second (2) electron on alternative levels of a local electronic center (see Local electronic levels) in a non-metallic crystal. Because of the mutual repulsion of electrons the relation U = E1 − E2 > 0 (positive correlation energy) is the usual one. The energy level positions and the charge states of the center for U > 0 are shown in Fig. (a, b) for a doubly-charged and an amphoteric center, respectively. The deformation of the atomic environment of the center caused by the strong interaction of the electrons with the atomic subsystem can give rise to a signiﬁcant increase of the potential well and the binding energy of the second electron on the center. In this case the relation U < 0 (negative correlation energy) becomes possible. Centers with a negative correlation energy are ﬁlled pairwise by electrons under the condition of thermodynamic equilibrium. In particular, if an amphoteric center concentration with U < 0 dominates, then one half of the centers are ﬁlled with pairs of electrons and have a negative charge, and the other half have a positive charge. The Fermi level EF thus is located in the middle between the donor and acceptor levels (Fig. (c)), and does not vary with a change in the concentration of the centers (socalled pinning). The amphoteric interstitial boron

Donor (D) and acceptor (A) energy levels between the top of the valence band (Ev ) and the bottom of the conduction band (Ec ) for positive (U > 0) and negative (U < 0) correlation energies, where EF is the Fermi energy.

atom in silicon is an example of a center with a negative correlation energy, another example is the Si V vacancy in silicon, where U < 0 for the trapping of the second electron on V − , and for the trapping of the second hole on V + . CORRELATION FUNCTION

The average of the product of several variables or functions corresponding to different points in space–time. Correlation functions describe the correlation of dynamic variable values. A correlation function or correlator of nth order is the quantity ξ1 (X1 )ξ2 (X2 ) . . . ξn (Xn ), where Xi = (xi , yi , zi , ti ), x, y, z are the space coordinates, t is the time; ξi is a dynamic variable or function, and stands for a certain averaging. In classical physics ξ(X) represents a random (often complex) ﬁeld, and the averaging is carried out over all possible ﬁelds under consideration. In the particular case when ξi depends only on time ξi = ξi (t) represents a random quantity, and the averaging is carried out over time. In quantum physics the ξi (Xi ) represent Heisenberg operators describing quantum ﬁelds, and the averaging is carried out over some state of the ﬁelds speciﬁed by the statistical operator (density matrix) ρ: ξ1 (X1 ) . . . ξn (Xn ) = Tr{ρξ1 (X1 ) . . . ξn (Xn )}. The Heisenberg operators can depend only on time, thus ξ1 (t1 ) . . . ξn (tn ) = Tr{ρξ1 (t1 ) . . . ξn (tn )}. An important case arises when the ξi represent operators for the creation

CORRELATION TIME

or annihilation of ﬁeld quanta (see Second quantization), or of particles (quasi-particles), or the quantum system as a whole in a certain state: ξi = ai+ or ai . In solid state physics these are creation and annihilation operators of electrons (holes), excitons, phonons, magnons, photons, or states of impurity centers (see Impurity atoms). In solid state quantum theory pair correlations ξ1 (t1 )ξ2 (t2 ), or second-order correlation functions ξ1 (X1 )ξ2 (X2 ), are the most widely used. When considering the pair correlator it is convenient to use average and difference times: t = (t1 + t2 )/2, τ = t1 − t2 , hence ξ1 (t1 )ξ2 (t2 ) = f (τ, t). Of fundamental importance is the spectral representation f (ω, t) = eiωτ f (τ, t) dτ which deﬁnes the system spectral characteristics. In the stationary case the dependence on t is absent. The pairwise temporal correlator f = a + (t1 )a(t2 ) in its spectral representation describes, through the frequency or the energy E = ω, the occupation of the state to which the operators a + , a are related. To evaluate the correlation function it is usually more effective to use the related Green’s functions. CORRELATION FUNCTION OF RANDOM FIELD

A statistical characteristic of a random ﬁeld (see Random potential) in a disordered system deﬁned by the equality ψn (r 1 , . . . , r n ) = V (r 1 ) . . . V (r n ), where n 2 is the order of these functions. Here 1 . . . n means averaging over the random ﬁeld Vr , and the origin of the energy scale is selected so that V = 0. Most widely used is the pair correlation function of a random ﬁeld ψ2 in terms of which many experimentally measured quantities can be expressed, such as the square of a random ﬁeld ﬂuctuation V 2 (r). In the Gaussian random ﬁeld case all functions ψn (n 3) are expressed in terms of ψ2 . In a macroscopically homogeneous disordered system the functions ψn (r 1 , . . . , r n ) depend only on (n − 1) differences r 1 − r n , r 2 − r n , . . .; and in particular, ψ2 (r 1 , r 2 ) = ψ2 (r 1 − r 2 ). An important property of random ﬁelds in real systems is the attenuation of correlations in systems at inﬁnity. With the distancing of the points r 1 and r 2 from each other the correlation of

217

the quantities V (r 1 ) and V (r 2 ) decreases. This provides an opportunity for the factorization of the average of the types V (R 1 ) . . . V (R n )V (r 1 ) . . . V (r m ) = ψm (r 1 , . . . , r m )ψn (r 1 , . . . , r n ), if R i = r i + α and |α| → ∞. In particular, ψ2 (r) → 0 as |r| → ∞. The distance |r 1 − r 2 | at which the pair correlation function ψ2 (r 1 , r 2 ) becomes and remains a negligible quantity is called the correlation radius or correlation length. This radius is an important characteristic length scale of a random ﬁeld, which determines the behavior of macroscopic quantities that depend on the ﬁeld. See Correlation length. CORRELATION LENGTH, correlation radius

The characteristic dimension of the region within which correlation between physical variables is appreciable. At distances exceeding the correlation radius these variables become statistically independent of each other, and their correlation function becomes equal to the product of their averages. Consider, e.g., a ferromagnet that is far from its critical point (transition temperature). The correlation radius is of the order of an interatomic distance. Thermal motions and quantum uctuations destroy the correlation of spin orientations at distances noticeably larger than this radius. As the critical point Tc is approached from above, the correlation radius grows, accompanied by the stronger and stronger cooperative effects that eventually result in the formation of a new ordered phase at T = Tc , and the material is ferromagnetic below Tc . CORRELATION TIME

Time interval τ during the course of which the value of the second-order correlation function decreases by the factor of e = 2.718. The stationary random quantity u(t1 ) (e.g., thermal displacement of the crystal atom) correlates with its value u(t2 ) at a later time t2 if the ensemble average value of the product c(t1 , t2 ) = u(t1 )u(t2 ) = 0. The quantity c(t1 , t2 ) is called the second-order correlation function. For stationary processes, e.g., lattice vibrations, c(t1 , t2 ) depends only on the time difference τ = t1 − t2 , and the dependence c(τ ) is such that |c(τ )| |c(0)|. For some classes of random quantities c(τ ) has an exponential dependence on τ : c(τ ) = c(0) exp(−τ/τc ), where

218

CORROSION

τ c is the correlation time, or the time constant associated with the relaxation decay of correlations. The quantity c(τ ) does not always have an exponential dependence on τ . For example, the single-phonon correlation function ui (t1 )uj (t2 ) is not exponential in the low-temperature region where the anharmonicity of vibrations is negligible (see Anharmonic vibrations), and its correlation time corresponds to the reciprocal width at half-maximum of the Fourier transform c(ω) = ∞ c(τ ) exp(iωτ ) dτ . −∞ CORROSION (fr. Lat. corrodo, gnaw away) Physicochemical interaction of a solid and a

medium (liquid, gas) resulting in the degradation of the material operating properties. During corrosion the oxidation of source material or its individual components (anode process) occurs with a simultaneous cathode process, i.e. the reduction of medium components by the uptake of electrons released at the anode reaction. Corrosion takes place irregularly on the surface due to the chemical and structural inhomogeneity of an actual solid body, and it is accompanied by product formation (including compact non-conducting depositions) from the elements present in the solid composition and surrounding medium. The local corrosion rate is limited by the rate of the slowest process, in accordance with the mixed electron potential on the surface (corrosion potential) which is being generated for conditions during which the rates of anode and cathode processes are equal. On the basis of the type of external exposure on the solid, which accelerates the breakdown process, we can distinguish electrochemical corrosion (during electric current ﬂow), stress corrosion, and photocorrosion (during illumination). In the latter case, for oxidation–reduction processes charge carriers are excited in the solid, and corrosion products participate in generating a new phase on its surface. There are external and internal photoeffects, such as the photoactivation of anode dissolution of n-type silicon, at a rate which is limited by the generation of holes at the Si surface layer. The nature of the surrounding medium determines different corrosion types: electrochemical, gas, atmospheric, soil, biological, sea, and so on. During high-temperature gas corrosion solid oxidation products (scale) are usually formed. In such

conditions the oxidizing agent diffuses through the scale to the solid surface, and solid components diffuse in the reverse direction. If the transport of components through the scale is impeded its primary layers show a protective, anticorrosion effect at the subsequent contact with the medium. The corrosion rate can be varied by introducing into the corrosion active medium some chemical compounds, e.g., inhibitors which decrease the rate of corrosion, or promoters which increase it. The protective mechanism of inhibitor molecules usually consists in their ability to diminish the limiting step rate of the corrosion process at adsorption on a solid surface, or to promote the formation of a protective coating which prevents corrosion (see corrosion protection). Volatile inhibitors which protect engineering industry products from atmospheric corrosion have gained wide-spread acceptance: corrosion inhibitors are added to lubricants, oils, fuel, brake ﬂuids, and emulsions that considerably decrease material losses from corrosion processes. The formation of anticorrosive coatings can also be promoted by alloying materials (steels) with special additives (Cr, Al, Si). CORROSION, CONTACT See Contact corrosion. CORROSION CRACKING Brittle failure of a metal in a corrosive medium

with a static ﬁeld of tensile stresses present in the lattice. The onset of corrosion cracking requires the presence in the medium of a component which creates the conditions for sharp localization of the corrosion process on the metal surface, and at structural defects. Corrosion cracking takes place in solutions of electrolytes (sulﬁde, chloride cracking, caustic embrittlement of steel, hydrogen cracking of steel in acid, etc.); in gases (hydrogen, ammonia), and in molten metals (mercury). A measure of a metal stability against corrosion cracking is its limiting tension loading with a particular base test, or more precisely, the critical coefﬁcient of stress intensity (cracking stability) KSI in the corrosion crack vertex below which the crack does not grow. The rate of crack growth is determined by the anode (active) metal dissolving rate in the crack vertex, the possible decrease of adsorption strength, hydrogen saturation of the

CORROSION OF METALS

metal volume before the crack, and the value of the stress intensity. The relative role of the corrosion factors differs for different metal–solution systems. In a hydrogen atmosphere at high temperature with cathode hydrogen saturation the main role is played by the hydrogen saturation of the metal, i.e. hydrogen brittleness. CORROSION FATIGUE

The degradation of a metallic crystal lattice in a corrosive medium at exposure to a variable ﬁeld of tension stresses. Corrosion fatigue is a measure of the limit of permissible cyclic metal loads in a given corrosive medium based on the number of selected load cycles, or on the critical intensity coefﬁcient of cyclic tension stresses below which the growth of cracks is not observed. The corrosion fatigue limit is much lower than that of metal fatigue in an inert medium. An increase of metal strength through a long-term base test, as a rule, does not cause an increase in corrosion fatigue in a given metal–medium system. Depending on the frequency and loading level, we can distinguish low-cycle and high-cycle corrosion fatigue. The types of loading are the stretching from zero, expansion–contraction, arching (pure and cantilever), torsion with different forms of loading cycles (sinusoidal, rectangular, trapezoidal, symmetric, asymmetric). Taking into account the presence of residual technology loading in real systems, the most general is asymmetric loading, which is also the most dangerous for a metal–medium system that is susceptible to corrosion cracking. Methods for limiting the increase in corrosion fatigue are the creation of compression stresses in the surface layers of a construction, surface alloying or use of protecting coatings, change of corrosion medium composition, lowering of the temperature, application of inhibitors, and electrochemical protection. CORROSION, INTERCRYSTALLINE See Intercrystalline corrosion. CORROSION OF METALS Metal destruction due to chemical or chemico-

physical interaction with a corrosive medium. A common cause of the corrosion of a metal (M)

219

is a chemical oxidizing reaction, e.g., by dry oxidizing gases in accordance with the following reaction: nM + mO2 = Mn O2m .

(1)

During the corrosion of metals in electrolytic media (electrolytic solutions, including those impregnated by porous bodies (e.g., soils), electrolytic melts) Mz+ cations transfer into the medium to form compounds with different solubilities. There are corresponding characteristic reactions in acidic and neutral aqueous solutions: M + zH3 O+ = Mz+ + 0.5zH2 + zH2 O,

(2)

M + 0.25zO2 + 0.5zH2 O = Mz+ + zOH− . (3) A metal–medium system, as a rule, is thermodynamically unstable, and hence it is an environment for the spread of corrosion. Despite successes in the development of materials with increased corrosion resistance, anticorrosive coatings, and other corrosion protection methods, the problem of metal corrosion persists because of the deﬁciencies of materials, the greater severity of the conditions imposed on metal usages, and other reasons. Economic losses from the corrosion of metals result from the decreased machinery and communications productivity, direct metal losses, and so on. In the case of the formation of thin ( Tc .

The formation of a Cottrell medium causes dislocations to become pinned. To separate dislocations from the impurity medium the stress σc ≈ W0 /b3 is needed, and σ0 ≈ 1 GPa for typical values W0 ≈ 0.1 eV. COULOMB EXPLOSION in a solid Expulsion of positive ions driven by Coulomb

Equipotential lines W (r, θ ) = const for an edge dislocation. Each circle is for a particular W0 value. The array of lines for c(r, θ ) = const is similar.

repulsion when several nearby atoms are simultaneously ionized. The Coulomb explosion may be caused by the simultaneous ionization of two atoms. The formation of an electron vacancy in an internal electron shell of an atom affected by ionizing radiation, or the appearance of a slow multicharge ion inside the solid or at its surface, can result in cascades of Auger transitions (see Auger effect). These may be both “vertical” in a single atom, and “horizontal” (when the growing positive charge is distributed among neighboring atoms, and ultimately results in a Coulomb explosion as well). A Coulomb explosion in a solid produces point defects, defect clusters can also form, and the surface of the solid may suffer sputtering. Coulomb explosions contribute to the degradation along the trajectories of heavy accelerated ions or fragments of nuclear ﬁssion. The Coulomb explosion in metals is not effective because of the rapid “dispersal” of microscopic positive charge in a metallic conductor. The rates at which charges

222

COULOMB GAP

are neutralized in insulators and semiconductors with their low concentration of current carriers are much slower, and the inﬂuence of the Coulomb explosion on the formation of defects may be much more effective. COULOMB GAP A gap in the density of states g(E) of electron excitations around the Fermi level μ in a disor-

dered system with localized electrons, e.g., the gap in weakly doped compensated or amorphous semiconductors that results from the long range Coulomb interaction. An important characteristic of the Coulomb gap is its energy Δ. Provided that the Coulomb interaction energy between two localized current carriers separated from each other by an average distance (averaged over all localized carriers) remains small in comparison with the characteristic spread of the energy levels, the 1/2 value of Δ is of the order of e3 g0 /ε3/2 in a three-dimensional system. Here ε is the dielectric constant, and g0 is the density of states at the Fermi level in the absence of the electron–electron Coulomb interaction (see Fig.). Such a situation is found in a crystalline semiconductor for both strong and weak compensation, and also in amorphous semiconductors. In the case of medium compensation in a weakly doped semiconductor Δ is comparable to the overall width of the impurity band, and the Coulomb gap is more strongly expressed. The density of states at the Fermi level vanishes only for zero temperature. With increasing temperature the Coulomb gap “closes” and totally vanishes as soon as the thermal energy kB T reaches several tenths of the value of Δ. This gap manifests itself in experiments that measure the

Density of states g(E) of an amorphous semiconductor near the Fermi level μ.

hopping conductivity versus hopping distance in

regimes where that the principal contribution to the electrical conductivity arises from states in the energy band that are within the energy range Δ from the Fermi level. A technique to observe the Coulomb gap directly is tunneling spectroscopy. COULOMB PSEUDOPOTENTIAL See Morel–Anderson Coulomb pseudopotential. COVALENT BOND, homopolar bond

A particular type of chemical bond formed between similar atoms or atoms whose properties differ very little from each other, when the pairing (overlap) of the electron shells of neighboring atoms takes place without any appreciable exchange of the electric charges of the two atoms. A typical example of a covalent bond is the bond in a hydrogen molecule. The two-electron wave function of such a molecule can be written down in the simplest Heitler–London approximation as follows: ψ(r1 τ1 , r2 τ2 ) = ψa (r1 )ψb (r2 ) + ψa (r2 )ψb (r1 ) × χa (τ1 τ2 ),

(1)

where ψa and ψb are the 1s-type one-electron wave functions centered on the a and b atoms, respectively, and χa is the antisymmetric wave function of the spins. The difference between the eigenenergy obtained from solving the Hamiltonian of the molecule constructed using the wave functions (1) and twice the electron energy in an isolated atom corresponds to the covalent bond energy. A similar construction is used for the wave function of two electrons of a σ -bond between nearest neighbor atoms in homopolar crystals (diamond, gray tin, germanium, silicon) as well as in the AIII BV and AII BVI compounds (ψa and ψb are distinguishable in this case, appearing as sp3 hybrid functions of the valence electrons of the atoms involved). If the crystal is formed from atoms belonging to different groups of the periodic system then there can be a greater or lesser admixture of ionic bond character in the bond, and this will be termed an ionic-covalent bond.

CRACK

COVALENT CRYSTALS Crystals held together by covalent interatomic

chemical bonds. Covalent crystals are most often formed by elements of Group IV and adjacent groups of the periodic system, and are characterized by a tetrahedral (sp3 ) hybridization of orbitals, with the chemical bonds formed by singlet pairs of electrons localized in the space between nearest neighbor atoms (see Covalent bond). Because these bonds display distinct direction and strength, covalent crystals posses a high hardness and elasticity, some of them being brittle. Covalent crystals usually exhibit a high thermal conductivity. The most typical covalent crystal is diamond (C); others are silicon (Si), germanium (Ge), gray tin (α-Sn), and a range of compounds formed from elements alongside group IV of the periodic system. These are: the AIII BV compounds, e.g., borazon (BN), GaAs, GaSb, InAs and AlP; AII BVI compounds, such as beryllium oxide (BeO), zinkite (ZnO), sphalerite (ZnS), CdTe, etc. All these compounds are semiconductors, with their energy band gap varying between 0.2 to 2–4 eV. As the elements move apart horizontally in the periodic system, like in the AI BVII compounds: CuCl, CuBr and AgI, the covalent nature of the bond weakens and it becomes partially ionic in character. Moving vertically down the periodic table some metallic features appear: for instance, crystals of white tin (β-Sn) are virtually metallic. Covalent crystals of triple and more complex compounds which likewise possess tetrahedral atomic coordination also exhibit some degree of metallic behavior; examples are chalcopyrite (CuFeS2 ), stannite (Cu2 FeSnS4 ), CdSnAs2 , etc. Covalent crystals with octahedral coordination are exempliﬁed by PbS, PbSe, SnTe, Bi2 Fe3 , Bi2 TeS2 , etc. Many crystals are heterodesmic (see Heterodesmic structures), i.e. the atoms in their crystalline structure have bonds of different types. Thus, graphite crystals are covalently bonded within the hexagonal layers, while the bonds between the layers are of the van der Waals type. The structure of elements close to Group IV, such as P, S, Se or Te, may be described in a similar way: the atoms form covalently bonded groups, but the groups themselves are bonded together by van der Waals forces. Many covalent crystals are widely used in technology: native and synthetic

223

diamonds as abrasives and silicon crystals of the highest purity serve as the basis of semiconductor electronics together with the covalent crystals Ge, GaAs, InSb, etc. COVALENT CRYSTALS, PLASTIC DEFORMATION See Plastic deformation of covalent crystals. COVALENT RADIUS

A parameter of the size of an atom in covalent compounds (see Covalent crystals). The covalent radius is deﬁned as half the distance between two identical atoms held together by a covalent chemical bond. The length of a single chemical bond between differing atoms can be evaluated as a sum of the covalent radii of the corresponding atoms. A commonly employed system is the set of Pauling covalent radii which are deﬁned for atoms in tetrahedral crystals such as diamond (C) and sphalerite (ZnS) (see Atomic radius). COVARIANCE

The quality of physical quantities found in reference frames of a certain theory being transformed to other frames according to representations of the invariance group of this theory. For instance, in special relativity Lorentz covariance presumes using physical quantities that transform as relativistic vectors (e.g., 4-vectors), tensors, spinors, etc. via Lorentz transformations. Gauge covariance is referred to in the case of a gauge transformation (see Gauge invariance). Covariance also implies the conservation of the form of an equation with respect to the transformations of the invariance group. For instance, the covariance of the form of the equations of general relativity implies that the equation appears the same in any four-dimensional reference frame, even though the speciﬁc equation coefﬁcients can (covariantly) change with a space–time transformation. CRACK

A disturbance of continuity of a solid which is localized along a certain surface; a plane defect with broken molecular bonds along its edges. There is a singularity at the crack tip which under mechanical loading leads to stress concentration

224

CRACKING

√ proportional to 1/ r where r is the distance from the crack tip. Depending on the shape of the displacement between the edges, cracks are classiﬁed as rupture cracks, and longitudinal and transverse shear cracks. In respect to stability, cracks are divided into equilibrium (i.e. subcritical which do not grow spontaneously) and nonequilibrium (i.e. overcritical which can propagate under action of the elastic potential accumulated by the system). In respect to the involvement of plastic deformation, cracks are divided into brittle (i.e. not connected with material yield) and tough (see Brittle failure, Tough failure) with a certain portion of plasticity. There are microscopic and macroscopic cracks. Classed among the former are sizes of cracks from the atomic scale to the subgrain scale. Referred to the latter are cracks whose dimensions are greater, by at least an order of magnitude, compared to the structural elements of the solid such as subgrains, crystallites, etc. The ﬁrst stage of failure is microcrack nucleation. There are two kinds of microcracks differing in the shape: elastic (force) cracks and dislocation cracks. The former are like an incision along an atomic plane with broken molecular bonds from one tip to another, and the surfaces are opened by the applied stresses. A particular feature of such a crack is its instability. It can spontaneously collapse after the stress release, so that it cannot exist in an unloaded body. A dislocation microcrack is an empty nucleus of a superdislocation with a large Burgers vector. It is mechanically stable, and can occur in an unloaded body. The nucleation of this type of crack is determined by collective dislocation processes. There is a series of crack nucleation mechanisms: dislocation junction, braked shear, opening of bent slip band, interaction of dislocations at crossing slip planes and at broken walls of subgrains, generation according to the scheme of opposite clusters and interacting twin layers, and so on. The second stage of microcrack development (subcritical growth) is also fully determined and controlled by dislocation phenomena. Its essence is the “falling” of dislocations in the crack that induces the growth of its Burgers vector. There are several mechanisms for this process: the crack is initiated by the slip band approaching a tip; two slip bundles adjoin the crack; an accumulation

in the crack of dislocations from the slip bands stopped by boundaries. At this stage of failure a substantial role is played by rotation processes when individual grains and their groups are able to rotate freely about the crack tip (see Plastic twisting deformation). Subcritical growth of the macroscopic crack proceeds via the same mechanisms with the added feature that the plastic deformation involving a large volume leads to the appearance of a system of secondary microcracks and pores prior to the main crack formation. The failure proper is then effected through a merging of the crack system into a common one by the tough rupture of bridges. The third stage of crack development, involving overcritical growth, proceeds with completely or almost completely suppressed plasticity at the vertex. Here, the spreading of the crack exhibits a distinctly elastic and overstructural character, with the limiting velocities of growth determined by the elastic constants of the medium, and by the sample geometry. The maximum possible velocities of failure, according to different evaluations, vary from 0.53 of the transverse elastic wave velocity to 0.38 of the longitudinal wave velocity. The limiting velocity of the crack, equal to the velocity of surface Rayleigh waves (see Surface acoustic waves) is considered to be the preferable index. In the case when additional feeding of the crack vertex by elastic energy is not mediated by the elastic waves that spread through the destructible material, but is performed directly, e.g., by plasma expansion at the vertex of crack under the effect of a laser beam, the velocities of crack propagation may be considerably higher, and may even exceed the sound velocity. See also Brittle crack, Nucleating crack, Submicrocracks, Tough crack, Wedge-shaped crack. CRACKING

The process of extraction of products with lower molecular mass from hydrocarbons, mainly of petroleum origin. The ﬁrst and foremost high tonnage industrial application of the process is extraction of motor fuels. Many processes of cracking are run in the presence of solid catalysts (catalytic cracking). The catalysts most often used are highly porous synthetic aluminosilicates containing Al2 O3 and SiO2 in various proportions.

CREEP

Complex sets of reactions involved in catalytic cracking always include the formation of new solid phases which poison the catalysts. These are cokes, and their mass can reach several per cent of the catalyst mass. To remove cokes the silicaaluminas are oxidized with air, or an air–vapor mixture (process of catalyst regeneration). CRACKING CORROSION See Corrosion cracking. CRACK RESISTANCE The same as Fracture toughness. CRAIG EFFECT (D. Craig, 1955)

Changes in the spectra of electronic and vibrational excitations of a molecule located in a crystal matrix. The inﬂuence of the local crystal e ld and intermolecular interactions results in a partial splitting of degenerate states, and changes of selection rules, thereby producing a larger number of observable bands in the optical spectra, and also changes their relative intensities and polarization properties. These phenomena were initially encountered during applied studies of molecular crystals. CREEP

Property of a solid to increase strain or to deform during the course of time under the action of a constant external stress or load, usually at an elevated temperature. The relationship between strain and time is given by the creep curve, which is arbitrarily divided into characteristic regions. At the moment of applying stress an instantaneous strain is induced; then comes the stage of initial creep or transient creep. The rate of deformation decays at this stage. At the second stage (secondary creep) the rate of deformation is constant. The third stage is characterized by an increase of the creep rate, then the process ends with failure. The shape of a creep curve depends on the temperature, stress, initial structure, and stability of the initial structure. Depending on these factors, there are four kinds of creep with different deformation mechanisms. (1) The ﬁrst kind of creep is observed if the applied stress is lower than the critical shear stress. This type of creep is called elastic creep or reversible creep. It is adequately described by the

225

equation ε = εl + ε0 [1 − exp(−t/τ )], where εl is a purely elastic strain (see Elasticity), t is the time after loading, ε0 and τ are constants. The second term of this equation stands for inelastic strain, which tends to ε0 . After load release the strain completely regains its value due to inelastic creep. One of the mechanisms, which provides an explanation for inelastic creep, proposes the diffusive transfer of impurity interstitial atoms into crystal lattice interstices, which are stretched under the action of the applied stress (see Diffusion). The strain ε0 is proportional to the applied stress, and to the concentration of impurity interstitial atoms. After release of stress interstitial atoms tend to become uniformly arranged at interstices, and the strain is restored. Inelastic creep may also be caused by short-distance transfer of dislocations, which does not involve abstraction from pinnings. (2) At stresses that are higher than the critical shear stress, the second kind of creep is observed in the low-temperature region, called logarithmic creep or low-temperature creep, and described by the equation: ε = α ln(1 + νt), where α 0 and ν 1 are constants. This relation is valid up to very slight strains (ε 0.2%). So far it is unknown whether logarithmic creep is followed by secondary creep, because tests to conﬁrm this are very time consuming to carry out. (3) As the temperature exceeds T G (for metals T G ≈ 0.5T melting and decreases with increased load) the third kind of creep is observed: high-temperature creep. The mechanism of hightemperature creep is related to the creeping of dislocations, and is controlled by processes that are determined by the rate of self-diffusion (motion of thresholds at screw dislocations, rate of creeping of dislocations around obstacles, etc.). High-temperature creep is described by the relation: ε = ε0 + βt m + Kt , where ε0 is the instantaneous strain, β and m are time-independent constants, 1/4 < m < 2/3 (according to Andrade (1910) m = 1/3), K and Kt are, respectively, the rate and strain at the ﬁrst stage. At this stage hardening dominates over dehardening, the density of dislocations increases, and the size of subgrains decreases; during the steady state the size of subgrains remains constant, whereas disorientation of subgrains increases in proportion to the increase of strain.

226

CREEP RESISTANCE

At the second stage of creep the duration and rate of deformation depend on the stress and temperature. The equation K = A exp[H /(k B T )] × sinh(Bσ )n , where T is temperature, σ is stress, A, B, n are constants, describes the temperature dependence and stress dependence of K. The activation energy H monotonically increases with the increase in temperature; for T > T G it is a constant equal to the self-diffusion activation energy. This means that at low temperatures diffusionrelated mechanisms of plastic deformation are activated. It has been found that slippage along the grain boundaries contributes signiﬁcantly to the creep at the second stage. The dependence of ε˙ is ∝ d 2 at low temperatures and ∝ 1/d at high temperatures, while at intermediate temperatures it takes the form k/d + Kd 2 , where k and K are constants, and d is the grain size. The inﬂuence of grain boundaries at elevated temperatures may be explained by localization of plastic deformation in border zones. The third stage of creep is prepared by structural changes, which take place at preceding stages. It is thought that acceleration of creep occurs because of an increase of stress that is related to the generation of a neck, the decrease of the actual cross-sectional area caused by accumulation of microcracks (see Cracks) and pores, or processes of recovery and recrystallization. (4) The fourth kind of creep, which is called diffusive creep, is observed at low temperatures and low stresses, and does not involve the transfer of dislocations, but is a result of directional diffusive mass transport. The rate of such creep, due to the self-diffusion or ﬂux of vacancies between external surfaces of the sample, has been calculated in works of F.R.N. Nabarro, C. Herring (1950) and R.L. Coble (1963). Taking into account the increase of creep rate caused by grain boundary diffusion, we obtain the equation: πδDg 5D σ Ω 1+ , ε˙ ≈ 2 Dd d kBT where D and Dg are the coefﬁcients of bulk and grain boundary self-diffusion, respectively, δ is the effective thickness of a grain boundary, and Ω is the atomic volume. Creep resistance of materials is characterized by the creep limit, i.e. the stress at which a certain

strain is achieved in a given time. Creep resistance depends on the type of interatomic bond, type of crystal lattice, stacking fault energy, grain structure, and other characteristics of the material. High creep resistance is the main factor determining the high-temperature strength of materials. See also Athermic creep, Diffusion mechanism of crystal creep, Radiation-induced creep. CREEP RESISTANCE See Creep. CRITERION OF LOCALIZATION See Anderson localization. CRITICAL CURRENTS in superconductors

The minimum value of the current Ic or current density jc at which the superconducting state is destroyed. Several types of critical currents are identiﬁed. In type I superconductors the value of Ic depends on the shape (geometry) of the sample. In particular, for a long enough cylindrical superconductor it is obtained from the condition that the azimuthal component of the magnetic ﬁeld of the longitudinal current, Bf = I /(2πa), reaches the value of the thermodynamic critical magnetic eld Bc (T ) at the surface of a sample of radius a. When I > Ic = 2πaBc (T ) the superconductor transforms to the intermediate state with a ﬁnite resistance. In type II superconductors the critical current density is determined by the pinning strength of the Abrikosov vortices, or by the ﬂuidity limit of the vortex lattice (see Vortex pinning). There is also a decoupling critical current at which the Cooper pairs are broken and the supercurrent ﬂow is terminated. The current velocity v = j/(eN0 ) (here j is the current density, N0 is the concentration of electrons in the metal) exceeds the critical velocity vc = Δ/pF , where Δ is the superconductor energy gap, and pF is the Fermi momentum (see Kinetic decoupling of Cooper pairs). Such currents may be reached in very thin superconducting ﬁlms and ﬁlaments, the magnetic ﬁeld of the current at their surface being lower than Bc (T ) in type I superconductors, or such that their thickness is smaller than the London penetration depth of the magnetic eld of a type II superconductor. However, recalling the presence of inhomogeneities, it becomes clear that

CRITICAL EXPONENTS

the destruction of the superconducting state, and the recovery of the resistive state in thin ﬁlms and ﬁlaments are usually controlled by vortex pinning at these inhomogeneities. Finding ways to increase critical currents is one of the most important tasks of applied superconductivity. CRITICAL DISORIENTATION OF DISLOCATION SUBBOUNDARY

The threshold value of the disorientation angle in a cellular structure at which, similar to grain boundaries, cell boundaries start to resist the movement of dislocations. The concept of critical disorientation of dislocation subboundaries resulted from comparing the mechanical properties of metals during the formation of the sublattice dislocation structure (either cellular or fragmented) that develops in the process of plastic deformation (see Fragmentation). While the overall density of dislocations remains unchanged with growing plastic deformation, they undergo redistribution in the process. The number of dislocations in the body of the subgrain diminishes, their density at subboundaries increases and the angle of disorientation of the adjacent cells grows, so that dislocation slip to large distances becomes more difﬁcult. The critical value of the angle of disorientation, θcr , usually remains within several degrees, and may be estimated from the expression Ky 2 (1 − ν)2 2πn θcr = , G 0.45b where G is the shear modulus, ν is the Poisson ratio, Ky is a constant value from the Hall–Petch equation (see Petch relation), b is the Burgers vector, n is the ratio of the effective slip length L to cell size l. Following the growing plastic deformation the number of subboundaries in the already formed dislocation cells increases, such that their disorientation angle is either equal to or already exceeds the value of θcr . This results in a signiﬁcant strengthening of the material, while the temperature of cold brittleness simultaneously decreases, which means that the formation of a disordered cellular dislocaton structure signiﬁcantly improves the overall mechanical properties of the material. For such a structure to form certain conditions have to be met, and the strain should take place within the temperature range of warm deformations.

227

CRITICAL EMBRYO, critical bubble

Seed or embryo of a stable thermodynamic phase in unstable equilibrium with its surrounding metastable phase (see Metastable state). The

radius of a spherical critical embryo is given by rE =

2γ v 2γ Tc (vM − v) = . μM (P ) − μ(P ) q(T − Tc )

Here γ is the coefﬁcient of surface tension; v, v M are the atomic volumes; μ and μM are the chemical potentials (see Thermodynamic potentials) for the embryo and the metastable phase, respectively; P is the external pressure, Tc is the phase equilibrium temperature; q is the latent heat of the phase transition from the metastable phase to the embryo phase. Only embryos above the critical size continue to grow. The process of growth, stable with respect to ﬂuctuations, sets in at r > r E + [k B T /(4πγ )]1/2 . For a supercritical embryo (r > r E ) to form it has to penetrate the thermodynamic potential barrier 4πrE2 γ /3. See also Nucleation at phase transitions, Crystallization. CRITICAL EXPONENTS, critical indices

Power law indices or exponents deﬁning the dependency of dynamic and thermodynamic parameters such as the external ﬁeld h, etc., on the reduced temperature, τ = T /Tc − 1, etc. around a second-order phase transition point (Tc ). Critical exponents only characterize the principal, leading asymptotes of these quantities. When τ, h change the system may pass through several regimes or phases, each of them described by its speciﬁc set of critical exponents. For example, when approaching the triple critical point the system passes through a transition region in which its behavior changes from that typical of a second-order phase transitions to a tricritical (around that point) behaviour. Critical exponents used to describe thermodynamic (statistical) properties of the system deﬁne the temperature dependences of the speci c heat cp ∝ |τ |−α , the order parameter M ∝ (−τ )β , the susceptibility χ ∝ |τ |−γ , and the correlation length rc ∝ |r|−ν , where the exponents β, γ , ν > 0. The critical exponents of anomalous dimensions for ﬂuctuations of the order parameter characterize the law by which the correlation func-

228

CRITICAL FLUCTUATIONS

tion decreases with distance r for r rc , G(r) ∝ r −(d−2+η) , where d is the dimensionality. For T = Tc the critical exponents describe the behavior of the system in the external ﬁeld h: cp ∝ h−ε , M ∝ h1/δ , rc ∝ h−μ (δ, μ > 0). Critical exponents are related to each other via certain algebraic expressions called scaling relations: α + 2β + γ = 2, βδ = β + γ , ε(β + γ ) = α, μ(β + γ ) = ν, ν(2 − η) = γ , γ d = 2 − α (see Scaling invariance hypothesis). Critical exponents also describe the kinetic (dynamic) properties of the system around Tc . For example, the relaxation time t (k, T ) of ﬂuctuations of the order parameter with wave vector k has the form t (0, T ) ∝ |τ |−y and t (k, Tc ) ∝ k −z in the critical region. Scaling relates these exponents to each other: y = zν. Critical exponents are universal values, i.e. they do not depend on the nature of the particular phase transition, or on the speciﬁcs of the physical system. They depend, instead, only on the number of components of the order parameter, and on the dimensionality d of the space. Critical uctuations become insigniﬁcant for d > dc , where dc is the so-called upper critical dimension, so that the critical exponents coincide with those provided by the Landau theory of second-order phase transitions. At d = dc ﬂuctuations generate multiplicative logarithmic corrections to the results from the Landau theory. If d < dc the corresponding critical exponents differ from those prescribed by the phenomenological theory of phase transitions. Their values may be (approximately) calculated using the techniques of high temperature expansions within the renormalization group method, in particular through expansions in powers of ε = dc − d (epsilon expansion), in terms of the spherical model, employing the 1/n expansion approach, and by other techniques. CRITICAL FLUCTUATIONS

Particularly strong thermodynamic ﬂuctuations of the order parameter and other physical variables observed near second-order phase transitions. The correlation length of these ﬂuctuations and their respective relaxation times grow without limit when approaching the transition point, thus reﬂecting destabilization of the corresponding phase, and the stronger role of the cooperative effects in forming the dynamics and thermodynamics of

the crystal. Much effort has been expended toward explaining the strong nonlinear interactions of critical ﬂuctuations (see Renormalization group method, Epsilon expansion). Experimental studies of critical ﬂuctuations by neutron diffraction, optical, radiospectroscopic, and other techniques yield rich data on the behavior of materials in the critical region. CRITICAL MAGNETIC FIELDS in superconductors

Values of applied magnetic ﬁeld strength (that depend on superconductor shape) above which the character of the penetration of the magnetic ﬁeld into the superconducting material changes, or the sample reverts to the normal (nonsuperconducting) state. One distinguishes between the thermodynamic critical magnetic eld Bc in type I superconductors (see Meissner effect), and the lower critical eld, Bc1 , the upper critical eld, Bc2 , and the third critical eld Bc3 in type II superconductors. See also Mixed states. CRITICAL PHENOMENA

Speciﬁc effects observed in the neighborhood of second-order phase transition points. One distinguishes between static and dynamic critical phenomena. Among the ﬁrst are the anomalies of the thermodynamics of crystals, and features in the behavior of static kinetic coef cients. Examples of static critical phenomena are: sharp increase in the magnetic permeability of ferromagnets as the phase transition point Tc is approached; anomalous temperature dependence of the speci c heat, elastic moduli, etc.; increase in the electrical conductivity of normal metals near superconducting phase transitions; and temperature anomalies in the speciﬁc heat of ferroelectrics. Dynamic critical phenomena involve the dynamic susceptibility, a sharp increase in relaxation times as Tc is approached (critical slowing down), anomalies in Raman scattering of light, in inelastic neutron scattering, in X-ray scattering, and in Mössbauer spectra (see Mössbauer effect). Sometimes critical phenomena are understood in a narrower sense, as effects produced speciﬁcally by critical uctuations of the order parameter. The susceptibility χ , the order parameter M, and the speciﬁc heat C, all behave as power law functions of the reduced temperature τ = (T − Tc )/Tc

CRITICAL STATE

around the critical point Tc : χ ∝ |τ |−γ , M ∝ |t|β , c ∝ |t|−α . Second-order phenomenological theory of phase transitions predicts the values α = 0, β = 1/2, γ = 1 for these power law indices called critical exponents, but it does not take ﬂuctuations into account. Experiments usually yield the ranges −0.1 < α < 0.1, 0.3 < β < 0.4, and 1.2 < γ < 1.4 for three-dimensional (non-layered, non-quasi-one-dimensional) systems. Speciﬁc values of the critical indices depend on the number of components of the order parameter. CRITICAL POINT

A point associated with a second-order phase transition. When the transition occurs during a temperature change the critical point corresponds to a critical temperature. Examples are the Curie point of a ferromagnet, and the Néel point of an antiferromagnet. The critical point can also be the value of an electric or magnetic ﬁeld which induces a change in phase, such as the upper and lower critical magnetic ﬁelds of type II superconductors. CRITICAL POINT, TRIPLE See Triple critical point. CRITICAL PORE SIZE Size of a pore in unstable equilibrium with

its surrounding environment. Smaller pores shrink and heal (see Healing of defects), while larger sizes grow. The critical radius of a spherical pore r cr depends on the coefﬁcient of surface tension γ , the density of point defects, their mobility, the nature of their elastic interaction with the pore (see Elastic interaction of defects), the gas pressure inside the pore and outside the sample, and other factors. For example, we have r cr = 2γ /[P + k B T N0 ln(1 + c/c0 )] in the presence of extra vacancies (vacancy concentration c, equilibrium concentration c0 ). Here P is the difference between the pressures inside the pore and outside the sample, k B is the Boltzmann constant, N0 is the number of atoms per unit volume of material. In polarized substances (with electric or magnetic moments) the pore tends to stretch along the moment direction. The equilibrium ratio of pore axes is determined by competition between the growing surface energy and

229

the diminishing ﬁeld energy as the lines of force ﬂatten, so that ratio grows for larger pore volumes. As the pore enlarges it sucks in more and more energy from the ﬁeld, and it eventually reaches the critical size V = V cr , where 1/3 Vcr = 0.476γ (ln(0.309/N 7/6 ))1/6 /(M 2 N 7/6 ). The principal axes of the demagnetization factor tensors of the sample and pore (see Demagnetization) are assumed to coincide. Here M is the moment per unit volume, and N is the principal value of the sample demagnetization tensor along the pore axis. As a rule, the segregation of impurities in the pore surface layer lowers the surface tension and results in a lower r cr . CRITICAL REGION, critical temperature range

A ﬂuctuational range in the neighborhood of a phase transition, located in the phase diagram adjacent to the second-order phase transition line, or to the critical point, where the thermodynamics and dynamics of the system are strongly affected by critical uctuations of the order parameter. The size of the critical region is characterized by the Ginzburg number, and depends on the type of interatomic (electron, spin) interaction potential associated with the phase. The behavior of the system in the critical region may differ both quantitatively and qualitatively from that predicted by the Landau theory of second-order phase transitions. CRITICAL STATE

The limiting equilibrium state of a two-phase system at which the physical differences between the two phases vanish. For example, the α- and γ -phases of cerium with the same face-centered cubic lattice become identical in the critical state. The “liquid–vapor” case is quite well known. The critical state on a phase diagram corresponds to a critical point or critical line. When approaching that point critical uctuations of the density of the substance become very much larger, while the latent heat of a rst-order phase transition approaches zero. At the critical point itself the phase transformation occurs simultaneously throughout the entire system, similar to a second-order phase transition. The values of the state parameters for the critical state are called critical parameters, e.g., critical temperature, critical pressure, critical volume.

230

CRITICAL STRAIN

CRITICAL STRAIN, critical degree of deformation The extent of strain that results in a qualitative

change in the behavior of a material under a given external action (e.g., deformation which produces sample failure), or an irreversible change of the sample shape (i.e. plastic deformation). Sometimes one may speak about a critical deformation with respect to certain physico-chemical characteristics of a solid, in particular about a critical plastic deformation resulting in recrystallization, etc. CRITICAL SUPERCOOLING FIELD The value of the magnetic eld Bs at which

a sample in a normal (i.e. nonsuperconducting) metastable state transforms into a superconducting state. A type I superconductor can be supercooled, meaning that it can remain in the normal state when the temperature is below the superconducting transition temperature T c , and the applied magnetic ﬁeld is also below the thermodynamic critical magnetic eld B c . A further lowering of the applied ﬁeld to the value B s brings about a phase transition to the superconducting state. The effect is only observed in pure (type I) superconductors, and its magnitude is characterized by the ratio α = Bs /Bc < 1. In some superconductors (Al, In, Sn, etc.) the extent of the overcooling may be quite signiﬁcant, and indium has been supercooled down to α < 0.1. CRITICAL TEMPERATURE

A temperature corresponding to a critical point, i.e. a point on a phase diagram at which the equilibrium curve for two phases in contact comes to an end. The concepts of critical temperature and critical point were introduced by D.I. Mendeleev (1860). The critical point is an isolated point of a second-order phase transition, and more generally Tc is often understood as the temperature of second-order phase transitions, including cases when the phase diagram contains a line or even a range of continuous phase transitions. The thermodynamic potentials of the system, which are functions of thermodynamic variables (such as temperature, volume, electric or magnetic polarization), feature singularities at T = Tc . While approaching Tc their derivatives, such as susceptibility, speci c heat, etc., may grow without limit. In the neighborhood of Tc the temperature dependences of thermodynamic variables are described

by power law functions (see Critical phenomena, Scaling invariance hypothesis). Several examples of critical temperatures are: transformation of a metal to a superconducting phase, transitions to magnetically ordered or ferroelectric states (Curie point), and transformation of a liquid to a super-

ﬂuid state. CRITICAL TEMPERATURE OF SUPERCONDUCTORS

Transition temperature Tc from the normal state of ﬁnite resistance R to the superconducting state of zero resistance, which is speciﬁc for each superconductor (see Fig.). In the absence of a magnetic ﬁeld the transformation corresponds to a second-order phase transition. For the phonon mechanism of superconductivity the value of Tc depends on the magnitude of the electron–phonon interaction constant λ. This interaction involves the attraction between pairs of electrons in the vicinity of the Fermi surface with the formation of Cooper pairs, despite repulsion from the Coulomb interaction. The calculation of Tc from ﬁrst principles is so complex that Tc is usually estimated from its dependence on various parameters in terms of simpliﬁed models. The most useful approach involves the Bardeen–Cooper–Schrieffer theory (BCS) which yields the following expression for Tc : Tc ≈ ΘD e−1/g . Here Θ D is the Debye temperature, and g is a dimensionless positive coupling constant, with the BCS model value given by g = N(EF )(Vph − Vc ), where N(EF ) is the density of states of electrons at the Fermi level EF , Vph and Vc are the

Critical temperature of superconductors.

CROSS-RELAXATION

matrix elements of the electron–phonon interaction (second order in perturbation theory) and the Coulomb repulsion, respectively. Note that g > 0 for Vph > Vc , corresponding to the BCS criterion for superconductivity. A more accurate accounting for the Coulomb repulsion in the energy range near EF results in its signiﬁcant weakening (the logarithm ln[EF /(ωD )] becomes large (see Bogolyubov–Tolmachyov logarithm) and a softening of the superconductivity criterion Vph > Vc∗ ≡

Vc . 1 + N(EF )Vc ln[EF /(ωD )]

McMillan (1968) was the ﬁrst to make approximate calculations of Tc for the cases of intermediate and strong coupling in the limit λ 1. He used the integral Eliashberg equations and obtained: ΘD 1.04(1 + λ) , exp − Tc = 1.45 1 − μ∗ (1 + 0.62λ) where μ∗ = N(EF )Vc∗ is the Morel–Anderson Coulomb pseudopotential. CROSS-DEFORMATION INTERACTION, electron–phonon interaction in one-dimensional metals Interaction between conduction electrons and long-wave phonons in conductors exhibiting onedimensional electrical conductivity (one-dimen-

sional conductors). It is produced by modulation of a random static scattering ﬁeld of impurities or other defects by a sound wave. It is non-diagonal in the electron momenta at the Fermi surface of a one-dimensional metal, i.e. the sign of the electron velocity can change due to this interaction. It is similar to the common deformation interaction (A.I. Akhiezer, 1938) that is described by introducing an additional term Hd = λik uik into the Hamiltonian of an electron, where the strain potential tensor λik is of the order of the Fermi energy, eF , and uik is the strain tensor. The cross-deformation interaction results in the appearance of a new term in the Hamiltonian, its structure schematically represented by Hcd = Δik uik , where Δik is the complex crossdeformation potential tensor. In the case of the weak scattering of electrons at impurities (defects), the cross-deformation interaction appears

231

much weaker than deformation scattering, meaning | ik |/λik ∝ (eF τ )−1/2 for eF τ 1, where τ −1 is the frequency of electron–impurity scattering. However, since the deformation potential in one-dimensional metals does not depend on the quasi-momentum of the electron at the Fermi surface, and the electron energy bands do not overlap, the Coulomb interaction between the electrons almost completely screens the potential λik (to the accuracy of terms in (qa)2 of the order of magnitude (qa)2 1, where q is the wave number of sound, and a is the crystal lattice constant). Therefore, alongside the inertial interaction resulting from the Stewart–Tolman effect, the crossdeformation interaction is the principal type of interaction of electrons with long-wavelength sound waves in one-dimensional metals (see Electron– phonon interaction). CROSS-LINKING OF POLYMERS See Polymer cross-linking. CROSSOVER TRANSITIONS See Direct transitions. CROSS-RELAXATION Relaxation processes in spin and other quan-

tum systems with non-equidistant energy levels that control the reestablishment of equilibrium between these levels after excitation by a radiation source. For example, consider a spin system with two resonant frequencies ωa and ωb , so that the difference between them does not exceed their line widths. The process of cross-relaxation develops via mutual spin ﬂips, the so-called spin-ﬂip process, resulting from the magnetic dipole interaction between the spins. It can also involve spin exchange. The extra energy (ωb − ωa ) released during cross-relaxation is compensated by the increase of the dipole–dipole interaction energy of the spin system. Cross-relaxation processes may involve two qualitatively different types of spin systems: resonant frequencies ωa and ωb for different types of spins (Fig. (a)); and frequencies ωa and ωb for one and the same spin type (Fig. (b)). The latter case can occur in a system with S > 1/2 under the inﬂuence of a crystalline electric ﬁeld. The rate

232

CROSS-SECTION

Examples of cross-relaxation processes.

of cross-relaxation depends strongly on the difference between the energies of the respective levels, and becomes negligible when this difference exceeds the average dipole–dipole interaction energy. This phenomenon was initially observed during nuclear magnetic resonance in LiF where the rate of transfer of resonance saturation from the Li7 nuclei to the F19 nuclei depends on the value of the applied magnetic ﬁeld. The process of cross-relaxation can decrease the spin–lattice relaxation rate of a slowly relaxing system of spins by coupling them with another spin system that relaxes more rapidly via a much shorter spin–lattice relaxation time. Cross-relaxation is thus a mechanism for thermal contact between the two spin systems. For example, slowly relaxing nuclear spins can transfer their energy to the lattice much more rapidly if they undergo cross-relaxation with rapidly relaxing electronic spins. Beside these two-spin cases, cross-relaxation processes may involve larger numbers of spins, such as during dynamic nuclear polarization. CROSS-SECTION of a process, effective cross-section

A factor characterizing the averaged rate of change in the state of particles as a result of their interaction (scattering, dispersion, chemical, nuclear and other reactions). Let the velocity of one of two interacting particles relative to each other be v. Consider a system of N (cm−3 ) ﬁxed and n (cm−3 ) particles moving with relative velocity v in some initial state, with their ﬂux characterized by the intensity Φ = nv particles·cm−2 ·s−1 . The cross section σ of the process of transition from the initial to the ﬁnal state caused by particle interactions is determined from the relation dn/dt = σ ΦN = γ nN , where t is the time, and

γ = σ v is the probability of an elementary act of the process. The cross-section σ at a given Nnv deﬁnes the fraction of particles undergoing the change: dn/n = σ Nv dt . The change caused by scattering is usually characterized by a scattering angle θ , by the change of scattering energy of the particles, or by the value of their orbital angular momentum l after scattering. In the case of nuclear or chemical reactions, the system after the reaction is deﬁned by the ﬁnal reaction products and their states. If it is necessary to determine the rate of reaction product formation by characteristics from an inﬁnitesimal interval of values, then differential cross-sections are used. For example, scattering in the interval of angles [θ, θ + dθ], and scattering with power transmission from the incident particle to the scatterer in the energy (temperature) interval [T , T + dT ], are characterized by the differential cross-sections dσ/dθ , dσ/dT , etc. The corresponding total cross-sections are σ = (dσ/dθ) dθ and σ = (dσ/dT ) dT , where the latter integration is from T = 0 to T = Tmax , representing the maximal energy transferred in the interaction. The cross-section is deﬁned by quantummechanical probabilities of transitions between initial and ﬁnal states of the system under the inﬂuence of particle interactions, or by reasoning from the classical mechanics equations of motion. Both the scattering cross-section and cross-sections of various reactions often differ appreciably from the geometrical cross-sections of the interacting particles, or from dimensions deﬁned by the radius of action of a short-range force, and they can be much larger or much smaller than the geometrical dimensions. Thus, the elastic scattering of particles on a ball of radius r is characterized in classical mechanics by the cross-section σ = πr 2 corresponding to the maximal geometrical ball cross-section. Quantum theory takes into account the wave properties of scattering particles, and provides the expression σ = 4πr 2 for λ r (λ is the de Broglie wave length, λ = h/p, p is the scattered particle linear momentum). For λ r the cross-section is σ = 2πr 2 , and the contribution to the total cross-section of the order πr 2 gives the small angle scattering. For resonant scattering the elastic scattering cross-section reaches the value σl = 4πλ2 (2l + 1), and for slow particles with λ considerably exceeding the radius

CRYOCRYSTALS

233

of action of the force it is much greater than the geometrical dimensions of the system. This effect has a quantum origin. The opposite situation with the cross-section much smaller than geometrical dimensions is realized in reactions where there is an energy potential barrier between the interacting particles. Then, on the average, repeated approaches of reacting particles are necessary to overcome the barrier. A similar situation often occurs in quasi-chemical reactions involving point defects in a solid. CROSS SLIP

A transition of helical sections of dislocations from one slip plane with the normal n, to another one with normal m, if the line of the intersection of these planes is parallel to the Burgers vector of the dislocation b, i.e. [n × m]||b. A slip plane is the closest packed plane of a crystal on which dislocations glide. The cross slip appears, ﬁrst of all, near the obstacles for the usual dislocation slip. If such an obstacle is local, then after the motion within the cross slip plane the dislocation may return to the initial plane, i.e. the process of double cross slip takes place. It is experimentally established that in face-centered cubic single crystals the beginning of the third stage of hardening is associated to the fact that as a result of the stress concentration by single or multiple steps there appear areas of dislocation lines which may perform cross slip. The process of cross slip determines the creep of metals in the interval of moderate temperatures (e.g., for aluminum single crystals within the temperature range 0 to 100 ◦ C). CROWDION (fr. crowd)

A speciﬁc quasi-one-dimensional point defect of the type of an interstitial atom such that adjacent atoms are preferentially displaced along one of the directions of dense packing. The extra atom in a crowdion in a fully packed row displaces 5 to 10 atoms along the line by individual minimal distances (much shorter than the interatomic distance a, see Fig.). H. Paneth (1950) introduced the concept of a crowdion to describe self-diffusion in alkali metals with BCC lattices (with crowdion direction 111). Experimental data are available proving the existence of crowdions in FCC metals (Cu, Ni) at low temperatures (along the 110 direction). A crowdion may form during radiation.

Crowdion.

A dynamic crowdion appears when a pulse sufﬁcient to displace a neighboring atom is transmitted along a fully packed atomic row to one of the atoms of the crystal. A relay displacement then takes place, and the crowdion propagates along the direction of the transferred pulse. A site vacancy remains at the site of the initially dislodged atom. A dynamic crowdion is able to propagate a distance of the order of 103 a from the position of the initially dislodged atom. A static crowdion may remain stable in some crystals within a certain range of temperature. It propagates as a whole, and the process involves one-dimensional diffusion along the atomic line. Although a crowdion can travel a long distance, the displacement of an individual atom at each step in the displacement process is the same (equal to a). In its quantum-mechanical description the crowdion is a quasi-particle (a crowdion wave). CRYOCRYSTALS

Solidiﬁed gases, i.e. crystals formed by atoms or small molecules with weak intermolecular interaction forces, which therefore feature low crystallization temperatures. Their relative simplicity is convenient for studies of the general properties of the crystalline state of matter. Atomic cryocrystals – solid Ne, Ar, Kr, Xe are closest to theoretical models of crystals with central force interactions. They form face-centered

234

CRYOGENIC TECHNOLOGY

cubic lattices containing identical atoms interacting via valence forces of attraction, and dispersion forces of repulsion. Their low-frequency collective excitations are phonons, and their highfrequency ones are excitons. Solid N2 , O2 , CO, CO2 , CD4 , etc., are molecular cryocrystals. Their molecules may be considered nondeformable since their intramolecular forces are much stronger than the intermolecular ones. Due to their rigidity these molecules rotate as whole units. Non-central interaction forces (dispersion, exchange, and multipole) result in certain orientations of these molecules in the crystal lattice. Phase transitions mainly arise from changes in that orientational order. Their collective excitations are phonons (both acoustic and optical); librons (which appear only when some long range orientational order exists); bound intramolecular vibrations; excitons, and their combinations. If the central interaction dominates over the noncentral variety (e.g., in solid CD4 ), the breakdown of long-range orientation order (orientation melting) occurs within the solid phase. Regions of short-range orientational order may still persist in orientationally disordered crystals. With increasing temperature these regions shrink, and librons transform into weakly perturbed rotations. Of particular interest is solid oxygen, a molecular magnetic substance with particular structural features and collective excitations (magnons, biexcitons) that result from the uncompensated electron spin of its paramagnetic O2 molecule. Quantum crystals form a separate group of cryocrystals (3 He, 4 He, H2 , HD, D2 and CH4 ). The dynamics of the translational and rotational motions of these molecules deﬁes a classical description, being controlled by the laws of quantum mechanics instead. The weak intermolecular interactions, small size, and light mass of these molecules all combine to produce properties typical of cryocrystals: low crystallization temperature, strength and thermal conductivity, and high plasticity, compressibility, vapor pressure, and thermal expansion coefﬁcient. CRYOGENIC TECHNOLOGY

Branch of technology involving the development, manufacture and use of instruments and machines that produce and maintain low temperatures, and that can liquefy and separate various

gases. Industrial applications of cryogenic technology are numerous, since pure oxygen obtained by liquefying air and separating its gases at low temperature is widely used in metallurgy and other industries. Liquid nitrogen, also obtained from liquid air, is more and more widely used for the longterm preservation of food products and biological materials, to operate transport refrigerators, for the needs of cryofracturing of various substances, etc. Various options of hydrogen liqueﬁers (up to 104 l/h), helium liqueﬁers (100 l/h), and refrigerators which reach millikelvin temperatures using 3 He dissolved in superﬂuid 4 He are manufactured. Cryogenic technology applies low-temperature methods to other technical areas, such as superconductivity. Using the phenomenon of superconductivity one may develop economically efﬁcient systems (e.g., large-scale magnetic devices with superconducting magnets for nuclear magnetic resonance imaging, accelerators, and thermonuclear installations). One may attain high speciﬁc power output for electric motors and generators, achieve very high sensitivities in measuring devices using the Josephson effect, etc. Projects are in progress to build superconducting electric power lines and transportation systems. CRYOGENIC TEMPERATURES

Low temperatures, in the range from 120 K to below 1 K (see Low-temperature physics). There exist various methods of deep freezing, or reaching these temperatures: cooling a gas when throttling (Joule–Thompson effect), isoentropic gas expansion in a gas expander, desorption cooling, expansion liquefaction, vapor pumping over a cooling agent, and so on. Combinations of two or more methods are often used. The liquefaction of nitrogen, hydrogen and helium provides the principal refrigerants in technical and scientiﬁc research. Vapor pumping over these liquids produces low temperatures in the range of 120–0.25 K (N2 ∼ 120–63 K; H2 ∼ 20–10 K; 4 He ∼ 4–0.7 K; 3 He ∼ 3–0.25 K). These refrigerants are employed in practice for cooling various electrical engineering devices (superconducting magnets, power transmission lines, electric generators, electric motors, transformers, etc.), electronic devices (radiation detectors, ﬁrst stages of ampliﬁers, computer elements, etc.) and

CRYOSTAT

other units. Deep freezing is used for gas blend separation, gas puriﬁcation, cooling of food, and for other purposes in medicine, construction, engineering, and so on. CRYOSORPTION (fr. Gr. κρυoς , cold, and Lat. sorbeo , absorb)

The process of absorption of gas from the environment by a strongly cooled solid or a cryogenic liquid called a cryosorbent. The removal from the gas phase by the liquid cryosorbent is called absorption. This process is explained by the ﬁnite solubility of certain gases in cryogenic liquids. A solubility coefﬁcient α (in m3 per ton of cryosorbent at 0 ◦ C and 760 mm Hg) is introduced. The value of α is a function of the partial pressure, P , and the amount of the absorbed gas is given by the expression σ = αP . The coefﬁcient α has a different dependence on the temperature for different materials. It decreases with the temperature if gaseous H2 or He is absorbed by liquid nitrogen; while for most gases absorbed by liquid methanol it grows with the drop in temperature. The absorption process is used in several separation cycles. During cryosorption of vapors by porous solids capillary condensation may occur. Cryosorption of vapors from certain multiphase gas systems may proceed by way of freezing the atoms of highly volatile fractions into a solid layer of a weakly volatile fraction precipitated at a cooled surface. A special case of cryosorption is adsorption of a material from the gas phase by a surface layer of a cooled adsorbent. The amount of gas, V , adsorbed by a unit mass of adsorbent depends on the nature of the adsorbent, and that of the adsorbed substance, and it grows for lower temperatures and higher gas pressures. The curve describing the dependence of V on P at T = const is called the adsorption isotherm. The amount of adsorbed gas is linear with pressure at low pressures, following Henry’s law: V = kP . As a rule, several processes proceed in parallel during cryosorption. Cryosorption is widely used in systems of vacuum cryogenic evacuation (see Low-temperature pumping methods).

235

CRYOSTAT (fr. Gr. κρυoς , cold, and σ τ ατ oς , standing, unmoving)

A device for cryostatting, i.e. for maintaining a constant cryogenic temperature between 0 and 120 K. Cryostats are used to study physical properties of materials, the phenomenon of superconductivity, to cool photodetectors, and to pursue other tasks at low temperatures. The simplest cryostat consists of two vacuum concentric bottles. The inner bottle, where the specimen under study is placed, is ﬁlled with a cryogenic liquid boiling at low temperature, e.g., with liquid helium (4.2 K). The outer bottle playing the role of thermal isolation is ﬁlled with a liquid boiling at a higher temperature, e.g., liquid nitrogen (77 K). Cryostats are often used to cool and store the specimen at a speciﬁc temperature within a wide range (from room to a very low value, e.g., 4.2 K). Such a device is not a cryostat in a strict sense, or is not one at every temperature. However, if its minimum attainable temperature falls within the cryogenic range, it is commonly called a cryostat. In most cryostats the sources of cold that absorb the heat removed from the specimen are liqueﬁed gases. The most widely used are liquid nitrogen (N2 ), helium (3 He, 4 He), hydrogen (H2 ) and, less commonly, oxygen (O2 ). Special cryostats used to cool photosensors sometimes contain solid noble gases. More recently compact refrigerators have been developed that can continuously pump a liquid or gaseous cooling agent into a cryostat. Together the two units form a joint cryostatting system. To reach superlow temperatures (T < 1 K) complex multistage devices are employed which achieve cryogenic temperatures of a specimen using liquid gases (3 He–4 He solution refrigerators), or through adiabatic demagnetization (see Adiabatic demagnetization cooling). Depending on the type of study, the cryostat may include optical windows (optical cryostat), a superconducting solenoid, a very high frequency lead, or other devices to probe the specimen in various ways. Many types of cryostats are available, varying in purpose, cooling technique, temperature range covered, permissible thermal load, accuracy, reliability, stability, character of probing, etc. Two main approaches have been followed in building cryostats:

236

CRYOTRON

1. Complex design for highly speciﬁc tasks, e.g., achieving extra low temperatures, cooling superconducting devices, cooling radiation sensors, solving problems in material development, etc. 2. Simple and cheap universal design for scientiﬁc and technological applications, to cover a wide temperature range, have short priming time, quickly reach functional range, have low maintenance cost, match well with peripheral measurement devices, permit manipulation of the cooled specimen, etc. Choosing the technique of heat evacuation from the specimen under study is of particular importance, especially for high heat inﬂux. Several common techniques for heat removal are: thermal radiation exchange, direct mechanical contact with the cooled surface, heat exchange through a gas carrier, the Swenson effect, and forced freezing of a target with a cold gas jet. These are all applicable over a wide temperature range, and have already reached advanced stages of development. The most widely applied cryostats make use of a single cryogenic ﬂuid, and are of two types, namely liquid immersion and stream ﬂow. To absorb thermal energy from the specimen liquid cryostats ordinarily use the heat of evaporation of a liquid coolant, but this only supports a temperature close to the boiling point of the coolant. Over a wide temperature range heat can be absorbed and removed via the speci c heat of a gaseous coolant. The temperature of a ﬂowing gas is easily varied, with the coolant brought directly to the specimen in the amount needed to compensate for the heat input from probing at a given temperature. Stream cryostats are of a more general nature, and permit using all the ﬁve known methods of heat evacuation immediately from the cooled specimen. Stream cryostats have several important advantages over the liquid type: they can achieve any temperature above the boiling point of the coolant; the coolant is very efﬁciently utilized; the temperature can be changed rapidly; the cryostat may be arbitrarily oriented in space; these cryostats are easily made small, etc. This small size capability is particularly important when matching cryostats to standard experimental devices, such as spectral instruments, optical or electronic microscopes, etc.

CRYOTRON

A superconducting device used as a switch, or a memory cell, in computers. Cryotrons employ the phenomenon of superconductivity turn-off by a magnetic ﬁeld. The current in an input circuit magnetically controls the superconductingto-normal transition in one or more output circuits. In practice a cryotron is a superconducting rod, or more commonly, a thin lm which may be in either the normal (switched-off) or superconducting (switched-on) state. A different superconductor with a higher critical ﬁeld controls it. The cryotron is switched from one state to another by varying the current through a control circuit. Cryotrons have the advantage that in their superconducting state the dissipation of energy in them is zero. An important characteristic is the switching time, which in more advanced designs may be as short as 10−10 s. CRYSTAL BASAL PLANE See Basal plane of crystals. CRYSTAL CHEMISTRY Branch of crystallography studying the locations of atoms and particles in crystals, and the nature of their chemical bonds. Crystal chem-

istry brings together the results from experimental X-ray and other diffraction techniques used to study the atomic structure of crystals (see X-ray structure analysis, Electron diffraction analysis, Neutron diffractometry), and combines them with both classical and quantum theories of chemical bonding to compute the energy of crystal structures, taking into account the crystal symmetry. Crystal chemistry approaches make it possible to explain, and in certain cases to predict, the positions of atoms and molecules in a crystal lattice, and their nearest neighbor distances, starting from the chemical composition of the material. Chemical bonding between atoms in crystals results from the interaction between their outer valence electrons. Depending on the nature of the bonding, the equilibrium distance between atoms is usually within 0.15–0.4 nm. When atoms are brought closer together than this a strong repulsion develops. Therefore, to a ﬁrst approximation, certain “sizes” or characteristic radii may be attributed to atoms for each type of bonding. Then

CRYSTAL CHEMISTRY

one may proceed from a physical model of a crystal envisaged as an atomic electron-dominated system, to a geometrical model that looks upon a crystal as an ordered arrangement of incompressible balls. A full crystal chemistry description includes specifying the size of the unit cell, the space group of the crystal, its individual atom coordinates, distances between them, and the types of chemical bonds that are present. In addition, the near environment of separate atoms, the characteristic atomic groupings, thermal vibrations of the atoms, etc., have to be taken into account. In terms of the type of their chemical bonding, crystals may be divided into four major groups: ionic crystals (e.g., NaCl), covalent crystals (e.g., diamond, silicon), metallic crystals (metals and intermetallic compounds), and molecular crystals (e.g., naphthalene). A certain structure is typical for each of these types of crystals. However, when thermodynamic conditions change these may sometimes alter (polymorphism). As a rule, the simpler the chemical formula of the compound, the more symmetric its structure. Crystals with identical chemical formulae (in the ratios of constituent atoms) may have identical crystal structures (identical structural types), despite possible differences in their bonding type (isostructure). Alkali halides of the NaCl type and certain oxides (e.g., MgO), as well as several alloys (e.g., Ti–Ni), are isostructural. Isostructural crystals with the same kind of bonding are called isomorphic (see Isomorphism). In many cases a continuous sequence of solid solutions exists between isomorphic crystals. The geometric model of crystals involves the concept of effective radii of atoms, molecules and ions (crystal chemical radii), so that their bonding distance is equal to the sum of such radii (additivity of crystal chemical radii). Using experimental data one can tabulate crystal chemical radii for all the types of bonding (see Atomic radii, Ionic radius). The principal geometric concept in crystal chemistry is the theory of dense packing that explains the positioning of atoms in certain metallic and ionic structures graphically. For ionic structures one may talk about “holes” in the packing of larger anions that are occupied by smaller cations of similar ionic radii.

237

The structural unit in molecular crystals is a molecule. Crystal chemistry of organic compounds considers the rules of dense packing of molecules, the relation between the symmetry of molecules and the symmetry of the crystal, and the types of organic structures involved. Speciﬁc crystal patterns are identiﬁed in the structures of polymers, liquid crystals, and biological crystals. The coordination number K (see Coordination sphere) and the type of coordination polyhedron characterize the chemical bonding of a given atom, as well as the structure of a given crystal as a whole. For example, Be (with a few exceptions) and Ge form a tetrahedral environment (K = 4), Al and Cr have an octahedron (K = 6) for their coordination polyhedron, and Pd and Pt are often square planar coordinated (K = 4). Low coordination numbers point to a signiﬁcant role of directional covalent bonds, and large K values (e.g., 6, 8, 12) indicate an appreciable role of ionic and metallic bonding. Bonds of various types coexist in many crystal structures (graphite, MoS2 , etc.). Such structures are called heterodesmic structures in contrast to homodesmic ones, the latter featuring uniform bonding (diamond, metals, NaCl, crystals of inert elements), and the former mixed bonding. The laws of thermodynamics determine whether or not a particular crystal structure will form. The structure most stable at a given temperature T is the one that has the lowest Helmholtz free energy F = U − T S, where U is the bonding energy of the crystal (energy needed to break up the crystal into separate atoms or molecules) at T = 0 K, and S is its entropy. The higher the free energy the stronger the bonding in the crystal. It is usually within 40–80 kJ/mol for crystals with covalent bonding, is somewhat lower for the molecular crystals, and is lowest for van der Waals bonding (4–15 kJ/mol). In practice, theoretically calculating the free energy and predicting the structure of crystals is only possible for comparatively simple cases. Such calculations can be carried out within the framework of the band theory of solids. In some cases semiempirical expressions for the potential energy of interaction of atoms in crystals can yield fairly accurate results for certain types of bonding (see Interatomic interaction potentials).

238

CRYSTAL CLASSES

Table 1. Meaning of the ﬁrst (I), second (II) and third (III) terms in the International Symbols of the 32 crystallographic point groups of the seven crystal systems (see ﬁgure). Crystal system

Position of each term in the symbol I

II

III

–

–

–

–

Trigonal

Unit symbol corresponding to any direction Twofold axis and/or reﬂection plane Twofold axis (x) or reﬂection plane Threefold symmetry axis

Hexagonal

Sixfold symmetry axis

Tetragonal

Fourfold symmetry axis

Cubic (isometric)

A symmetry element

Triclinic Monoclinic Orthorhombic

CRYSTAL CLASSES

Crystallographic classes or symmetry classes are categories of crystallographic point groups of symmetry (introduced in 1830 by J. Hessel and, independently, by A.V. Gadolin in 1867). To denote crystal classes symbols are used (see Crystal symmetry) that are based on group theory theorems for the combination of symmetry operations. According to these, the product of two symmetry elements produces another element of the symmetry group. Table 1 presents notational rules for crystal classes that are found in various crystallographic systems. For example, the point group 43m corresponding to the mirror plane class of the cubic system, denoted by Td (dihedral-tetrahedral) in the Schönﬂies system, has a fourfold inversion axis (4), a threefold rotation axis (3) and a mirror plane (m). The axial monoclinic point group (Schönﬂies C2 ) has only a twofold axis. The coordinate and diagonal elements of symmetry are understood as planes and axes passing along the coordinate planes (axes) and the bisectors of the angles between them, respectively. The crystal classes are separated into primitive (single symmetry axis), centric (symmetry axis plus center of symmetry), planar (n symmetry planes along the axis), axial (having n twofold axes normal to the symmetry axis), etc. Elements of the crystal

Twofold axis (y) or reﬂection plane Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane Diagonal threefold axis

Twofold axis (z) or reﬂection plane – Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane Possible twofold axis or reﬂection plane

classes of the 32 crystallographic point groups are presented in the ﬁgure. CRYSTAL CLEAVAGE The capacity of monocrystals to be split

(cleaved) along certain crystallographic planes (crystal cleavage planes) on exposure to a mechanical force or impact. The cleavage is related to the speciﬁc features of the crystal structure. The crystal is split along directions or planes of smallest crystallographic indices, which involves the breakage of the weakest bonds. Thus, the graphite structure is susceptible to actions counteracting van der Waals forces perpendicular to (0001), which involves the separation of adjacent sheets of carbon atoms from one another. Most cubic crystals cleave along cubic planes. The crystal cleavage plane of BCC metals is often (100), whereas hexagonal crystals cleave along the basal plane. The orientation of the cleavage planes of certain crystalline materials (e.g., sphalerite) is determined by the charge of adjacent separable atomic sheets. Cleavage along planes of opposite charge requires more energy than splitting along planes containing ions of the same sign. The following degrees of cleavage of crystals are distinguished: highly perfect cleavage (cleaved into thinnest layers), perfect cleavage (crystal split

CRYSTAL DETECTOR

into bars along cleavage plane), average degree of cleavage (cleavage facets accompanied by randomly shaped facets), imperfect cleavage (fractography patterns exhibit mostly macroscopically irrational fracture regions), completely imperfect cleavage (practically no cleavage: fracture is conchoidal). Cleavage is one of the characteristic properties of a crystalline material. It is helpful for the determination of a crystal disorientation. Surfaces of high perfection, exposed on splitting along the crystal cleavage plane, are convenient for study. The phenomenon of crystal cleavage is used in jewelry trades to prepare a gem for its crystal faceting.

239

CRYSTAL DETECTOR, crystal counter

An instrument to record and analyze spectroscopic properties of nuclear particles and photons. The crystal counter is an electric capacitor (usually parallel plate type), ﬁlled with a single crystal insulator (e.g., diamond or CdS). A charged particle entering the dielectric produces ionization along its path, and free current carriers appear which are driven to the capacitor electrodes by the external electric ﬁeld. A short electric pulse results, its amplitude proportional to the energy released by the particle in the crystal. After ampliﬁcation it is recorded by a counting device or amplitude analyzer.

240

CRYSTAL DIFFRACTION SPECTROMETERS

Simplicity of design and maintenance, small size (below 1 mm2 ) and the fact that certain crystals, e.g., diamond, can function at high temperatures, make crystal counters convenient nuclear radiation detectors that are widely used in physics, dosimetry, various industrial applications, etc. CRYSTAL DIFFRACTION SPECTROMETERS

A class of X-ray spectral instruments for studying absorption and emission spectra of matter and the structural features of monocrystals. Crystal diffraction spectrometers may be single-axis (sample crystal), double-axis (collimator crystal plus sample), and triple-axis (collimator, sample, and analyzer crystals) types. As the number of elements in the instrument grows, its spectral dispersion and angular divergence of the radiation diminish, so that it becomes possible to better expand the diffracted intensity over the angle. Single-axis diffraction spectrometers are only capable of measuring the integrated intensity of the diffraction. Double-axis instruments can record X-ray spectra or rocking curves for monochromatic radiation (i.e. dependence of diffracted intensity on X-ray angle of incidence). They also provide for antiparallel and parallel positioning of the crystals so that the resulting dispersion is either doubled after the beam passes through the sample crystal, or it reverts to zero. The ﬁrst position is used for spectral studies, and the second (zero dispersion) for structural studies during which the width and intensity of the diffraction maximum are measured. Triple-axis spectrometers permit the separation of the coherent component of the integrated intensity from the diffuse one. See also X-ray spectrometer. CRYSTAL FACETING, crystal cut

Outward shape of crystals speciﬁc for a given crystal class. Faceting conforms strictly to the

point group symmetry relationships of a crystal (see Crystal symmetry), and only includes faces of certain categories, the so-called simple forms (see Crystal polyhedron). As a rule, the simple forms that are possible within a given point group symmetry tend to display various combinations one with another. The shapes of individual crystals are closely related to their structure. Materials without

clearly preferred directions form, as a rule, uniformly developed isometric polyhedra. The acicular crystals are typical of materials with needlelike or chain structures; plate-like crystals are typical of materials with laminated structures, and so on. In most cases, the only crystal faces that participate in the crystal faceting are those parallel to crystal lattice planes of the structure. The latter possesses high reticular density, i.e. their unit area maximizes the number of particles (Bravais law). In an ideal case the faces of each simple form must have the same conﬁguration and dimensions. The shape of a real individual crystal is determined by the speciﬁc conditions of its growth: temperature, pressure, concentration, impurity atoms content, etc. When characterizing the crystal faceting, the terms form and habit are commonly used. The former term concerns a general view of a polyhedron (isometric, acicular, ﬁbriform, etc.), while the latter serves to describe the outward appearance of the individual crystal with the help of dominant simple forms (octahedral, prismatic, dipyramidal, and so on). CRYSTAL FIELD, internal crystal eld, crystalline electric eld The electric ﬁeld at a point within a crystal,

produced by its atoms or ions. This ﬁeld determines energy level splittings of atomic electronic conﬁgurations, and the periodic potential of the crystal ﬁeld determines the band structure of the crystal for an ideal lattice corresponding to the crystallographic space group. An impurity ion (or local ionic center) has an energy spectrum determined by the local crystal ﬁeld symmetry. The internal electric ﬁelds of defects bring about an inhomogeneous broadening of the spectral lines of resonant transitions. The line shape (proﬁle) depends on the nature of the defects and their distribution within the crystal. To compute the shape of the resonance lines one can use statistical theory of line shape, or possibly the method of moments. Crystal eld theory is applied in various branches of physical science (optics, radiospectroscopy, etc.) to calculate the energy transitions responsible for spectra. It considers various models of the ﬁeld, and basically accounts for the spatial motions of electrons and nuclei. Energy level splittings produced by the crystal ﬁeld generally

CRYSTAL FIELD THEORY

lie in the optical frequency range (1013 –1015 Hz). Accounting for the spin variables along with the spatial degrees of freedom results in an additional splitting or shifting of the levels. The crystal ﬁeld affects the spin through the spin–orbit interaction. Spin level splittings may be treated using a framework similar to crystal ﬁeld theory called the spin Hamiltonian technique. The energy level spacings associated with electron spin interactions lie in the frequency bands of electron paramagnetic resonance (108 –1011 Hz), while those resulting from the nuclear spin are 2 to 3 orders of magnitude smaller, the same as the frequency range of nuclear magnetic resonance. CRYSTAL FIELD GRADIENT

A symmetric second-rank zero trace tensor with components equal to the second derivatives of the potential V (r) of the electric ﬁeld at the site of an atom or ion in a crystal: Vαβ = (∂ 2 V /∂xα ∂xβ )|r=0 . The crystal ﬁeld gradient deﬁnes the energy H of the quadrupole moment Qαβ of a nucleus (see Quadrupole), located at the site: (2) Qαβ Vαβ = Qm V−m , H= αβ

m

(2)

where Qm are the components of the tensor operator of the nuclear quadrupole moment: 1 Vzz , 2 1/2 1 V±1 = ± (Vxz ± iVyz ), 6 1/2 1 V±2 = (Vxx − Vyy ± 2iVxy ). 24 V0 =

The crystal ﬁeld gradient of the tensor Vαβ in a system with two principal axes is characterized by two independent parameters eq = Vzz and η = (Vxx − Vyy )/Vzz , where |Vzz | |Vyy | |Vxx |, the dimensionless asymmetry parameter η is limited to the range 0 η 1, and the Hamiltonian of the quadrupole interaction assumes the form −1 H = e2 qQ 4I (2I − 1) × 3Iz2 − I (I + 1) + η Ix2 − Iy2 ,

241

where q is the quadrupole moment of the nucleus with a spin I 1. The crystal ﬁeld gradient for cubic symmetry is zero. When calculating a crystal ﬁeld gradient one has to take into consideration the ﬁelds of point charges (lattice summation carried out by the Ewald method), and the multipole moments of ions and conduction electrons. To take into account the polarization of the full electron shells of an ion in the crystal e ld, its ﬁeld gradient at the nucleus is written in the form (1 − γ )Vαβ , where γ is the antiscreening factor. For most ions the value of γ is within the range from −10 to −100. CRYSTAL FIELD SPLITTING See Bethe splitting. CRYSTAL FIELD THEORY (H. Bethe, 1929) Theory describing electronic states of ions with unﬁlled d- and f -shells in crystals. The scope

involves such areas as optical spectroscopy, magnetic properties, and mechanisms of the electron– phonon interaction, in crystals containing ions of the three transition metal groups, the lanthanides, and the actinides. Crystal ﬁeld theory treats the splitting of electronic energy levels of localized dand f -electrons by an effective internal crystalline ﬁeld. The Hamiltonian is solved using perturbation techniques for a single conﬁguration, with the states of a single electron in the central ﬁeld of a free ion taken as the zero-order approximation. The perturbation operator deﬁned in the space of the wave functions of the (nl)N -shell equals the sum of the energies of the electrostatic interaction, Hee , the spin–orbit interaction, H so , and the energy of the electron in the crystal ﬁeld, Hc . The Hamiltonian, Hc is averaged over the radial distribution of electron density, and has the form: Hc =

N i

(k)

(k)

Bqk Cq (i),

kq

where Cq (i) are spherical operators in the space of angular variables of the ith nl-electron, and Bqk are the crystal ﬁeld parameters, quantitative characteristics of the potential of the electric ﬁeld at the paramagnetic ion site in an equilibrium conﬁguration. They have dimensions of energy, are generally complex, and satisfy the relations

242

CRYSTAL FIELD THEORY

k . The number of independent Bqk ∗ = (−1)q B−q parameters depends on the symmetry of the crystal ﬁeld, while the structure of the operator Hc is determined by the choice of local coordinate system. For example, a cubic crystal ﬁeld has the octahedral point group of symmetry Oh . In the system of Cartesian coordinate axes coinciding with the C4 symmetry axes the Hamiltonian of the electron interaction with the cubic crystal ﬁeld is given by 5 (4) (4) (4) C + C−4 H = B4 C 0 + 14 4 7 (6) (6) (6) + B6 C 0 + C4 + C−4 . 2

The even component of the crystal ﬁeld potential is the same in the case of tetrahedral (Th , Td ) coordination. Often the cubic symmetry component dominates at a low-symmetry site. The parameter 10Dq = (10/21)B4 equals the difference between the two d-electron energies in a crystal ﬁeld of cubic symmetry (doublet eg and triplet t2g states), and provides a measure of the ﬁeld “strength” for ions with partially ﬁlled d n -shells. The f n -shell multiplet splittings in cubic symmetry are deﬁned by the parameters B4 and B6 , and the structure of the wave functions of the respective states depends on only a single parameter (x), proportional to the ratio B4 /B6 . The effects produced by the spatial correlation of electrons, and the change of the electrostatic interaction parameters in the crystal ﬁeld, are described by a two-term operator: (k) (k k )k (2) C (k1 ) (i) × C (k2 ) (j ) Bq Bq 1 2 , Hc i>j

that has a complex tensor structure. The parame(k k )k ters Bqk , Bq 1 2 can be evaluated from optical or magnetic measurements, or computed within various crystal ﬁeld models. Quantum-mechanical calculations taking into account the electron structure of the nearest neighbors of a paramagnetic ion are sometimes called ligand ﬁeld theory. When calculating the energy spectrum of the (nl)N electron shell one should distinguish between strong crystal ﬁelds (ions of 4d and 5d transition groups, Hc > Hee > Hso ), intermediate ﬁelds (ions of the 3d iron group, Hc ∼ Hee > Hso ), average ﬁelds (Hee > Hc > Hso ), and weak ﬁelds (rareearth elements, Hee > Hso > Hc ). Various options

for constructing the matrix of the Hc operator depend on the choice of the basis for the zeroth approximation (e.g., single electron wave functions, functions of terms |γ LSML MS , or functions of multiplets |γ LSJ MJ ). Piezospectroscopic or electric ﬁeld effects in the spectra of paramagnetic crystals can result from changes in the crystal ﬁeld during corresponding external actions on the lattice. Modulation of the crystal ﬁeld by lattice vibrations is the principal mechanism of the electron–phonon interaction. Crystal ﬁeld models help with computational techniques. The simplest and historically the ﬁrst point charge model envisaged the crystal lattice as a collection of point charges Qλ e located at lattice sites (λ labels the site), with the charges themselves prescribed by the valences of the respective ions. To determine the ﬁeld of point charges one has to calculate the lattice sums: 1/2 4π k q e2 r k Bq = −(−1) 2k + 1 ×

k (θ ϕ ) Qλ Y−q λ λ λ

Rλk+1

,

where Yqk are spherical harmonics, rλ , θλ , ϕλ are the spherical coordinates of site λ (the paramagnetic ion is at the coordinate origin), and r k are the moments of the electron radial density in the unﬁlled shell. Discrepancies of an order of magnitude often exist between calculated and measured crystal ﬁeld parameters. To account for this one may consider changes in the radial density of the d- and f -electrons in the crystal ﬁeld, ﬁelds of point multipole moments (dipoles, quadrupoles), the distribution of charges of lattice ions, screening of f -electrons by the outer ﬁlled electron shells, etc. The electronic structure of selected complexes that include the paramagnetic ion and its nearest neighbors (ligands) immersed in the crystal is treated by cluster models (see Cluster). Electron energies in the complex are calculated using a one-electron Hamiltonian that operates in the space of molecular orbitals (LCAO method, see Molecular orbital), or in the space of mixed conﬁgurations. Charge transfer from the ligands to the paramagnetic ion is also taken into account (the Heitler–London approximation). To

CRYSTAL LATTICE

simplify estimates of matrix elements of the oneelectron Hamiltonian (see Single-electron approximation) one uses either the Mulliken–Wolfsberg– Helmholtz method (R.S. Mulliken, M. Wolfsberg, G. Helmholtz, 1952) or the local exchange potential (Xα -technique). The dominant role in forming the energy spectrum of the cluster and the corresponding potential of the effective crystal ﬁeld involves effects produced by the overlapping of the spatial distributions of charges of the ligands and the paramagnetic ion. Among such effects are the Kleiner correction to the Coulomb ﬁeld of the ligands, the exchange interaction, the mutual nonorthogonality of wave functions of the ligands and the metal ion, covalency, virtual excitations of the cluster accompanied by charge transfer from the ligands to the paramagnetic ion, followed by the formation of holes in its ﬁlled electronic shells. One may explicitly determine the interrelations between the composition and structure of the crystal lattice, on the one hand, and the energy spectrum of the paramagnetic ions on the other, using semiphenomenological models that involve a limited number of parameters determined from experimental data. The energy of an nl-electron in an axially symmetric ﬁeld of the ligand λ is

k (k) equal to Hc(λ) = k B 0 (Rλ )C0 (quantization axis parallel to r λ ). Assuming that individual ligand ﬁelds may be summed, and using the power k −t series approximation B 0 ∝ Rλ k , one may express the terms of the crystal ﬁeld through four (k = 2, 4 for l = 2) or six (k = 2, 4, 6 for l = 3) parameters of the “superposition model” k B 0 , tk . To parameterize the spectra of paramagnetic ions using the model of angular overlap and the model of exchange charges it is sufﬁcient to k represent the functions B 0 (Rλ ) by linear combinations of squared overlap integrals of the wave functions of the d- (or f -) electron with the ligand wave functions. Satisfactory models are still lacking for rare-earth metals and actinide compounds. The so-called odd components of the crystal ﬁeld are treated separately since they mix together the states of different parity that correspond to the ground state ((nl)N , 1 = N < 2(2l + 1)), and to the excited ((n l )4l +1 (nl)N+1 , (nl)N−1 (n l )) electronic con gurations of the ions of rare-earth and transition metals. The energy of a localized

243

electron in an odd crystalline ﬁeld corresponds

2p+1 2p+1 to the Hamiltonian H = Bk Ck , deﬁned in the subspaces of one-electron functions 2p+1 n l ml |, |nlml with their parameters Bk (where 0 p (l + l − 1)/2) different from zero when the point group of symmetry of the ion does not include inversion. The odd components control the intensities of the dipole transitions between the states of an unﬁlled (nl)N -shell (forbidden for free atoms), as well as the linear electric eld effects in optical spectra and the spectra of paramagnetic crystals. When perturbation theory is applicable one can introduce an effective operator (H A + AH )/Δ instead of the odd single particle operator A in the space of states of the basic electron conﬁguration. Here Δ is the average energy difference between the excited and ground state conﬁgurations. Additional terms in the effective operator of the dipole moment proportional to the squared electron radius (r 2 ) are called pseudo-quadrupole moments. Calculating the Stark structure of the spectrum of the unﬁlled shell, the effective even ﬁeld H 2 /Δ is allowed along with the even component of the crystal ﬁeld. The odd components, induced by odd vibrations, deﬁne the intensities of the electron– vibrational transitions between the states of the same parity for ions in the crystal lattice sites, the latter also serving as the centers of symmetry. CRYSTAL GRAINS See Polycrystal. CRYSTAL, IDEAL See Ideal crystal, Perfect crystal. CRYSTAL LATTICE

A geometrically ordered arrangement of atoms (ions, molecules) typical of the crystalline state of matter (see also Lattice). The geometry of an ideal crystal involves a spatial periodicity (translational symmetry, see Crystal symmetry) characterized by three noncoplanar basis vectors a j (j = 1, 2, 3) such that the displacement of the lattice by a vector n1 a 1 + n2 a 2 + n3 a 3 (n1 , n2 , n3 are integers) brings it into itself. If every a j is selected to be the shortest possible displacement in its respective direction, the parallelepiped formed by the three

244

CRYSTAL LATTICE BASIS

basis vectors is called the unit cell or the primitive parallelepiped. By simply replicating the unit cell in space one may generate the entire crystal structure. The choice of the set of a j vectors is not unique; yet the unit cell volume is independent of such a choice. If a unit cell can be chosen so that it contains only a single atom then it is called a primitive cell. All other unit cells are called nonprimitive cells. A complex crystal lattice may be envisaged to consist of one or several Bravais lattices ﬁtted into each other, each such Bravais lattice being built of atoms of a single type. The presence of a crystal lattice explains the phenomenon of anisotropy of crystals and crystal faceting. Experimentally, crystal lattices can be identiﬁed and classiﬁed by X-ray, electron, and neutron diffraction techniques. CRYSTAL LATTICE BASIS, unit cell basis

Set of atoms and their coordinates with the same location at each point of a Bravais lattice. By adding the basis to the Bravais lattice, one obtains a crystal lattice structure. CRYSTAL LATTICE CONSTANTS

The magnitudes of three noncoplanar translations (a, b, c), by which the Bravais lattice may be constructed for a given crystal. The lattice is to satisfy three main conditions: (1) the symmetry of the lattice unit cell must correspond to the microscopic crystal symmetry; (2) the unit cell is to possess the highest possible number of right angles (or the highest possible number of equal angles and equal sides); (3) the unit cell is to have a minimal possible volume (with due regard for the conditions (1) and (2)). The set of crystal lattice constants (a, b, c) and the angles between them: α (between b and c), β (between a and c) and γ (between a and b), is called the crystallographic basis. There are seven types of crystallographic basis sets that correspond to the seven crystallographic systems, as follows: • a = b = c, α = β = γ = 90◦ , cubic system; • a = b = c, α = β = γ = 90◦ , tetragonal system; • a = b = c, α = β = 90◦ , γ = 120◦ , hexagonal system; • a = b = c, α = β = γ = 90◦ , trigonal system;

• a = b = c, α = β = γ = 90◦ , orthorhombic system; • a = b = c, α = β = 90◦ , γ = 90◦ , monoclinic system; and • a = b = c, α = β = γ , triclinic system. CRYSTAL LATTICE DYNAMICS

The branch of solid-state mechanics, which studies the internal movements within a crystal, taking into account the discreteness of its atomic structure. It includes the classical and quantum mechanics of collective movements of atoms in an ideal crystal, the theory of interactions of the crystal with penetrating radiation, and also the dynamics of imperfect crystals. Due to the strong chemical bonding the internal motion cannot be described as the superposition of independent displacements of separate atoms. If the displacements are small and the harmonic approximation applies then normal vibrations occur, each of which involves the participation of all the atoms. The normal vibration has a form of a plane wave characterized by the wave vector k, expressed within the ﬁrst Brillouin zone, which determines the direction of propagation of the wave front, with wave length λ = 2π/|k|, and a polarization vector which indicates the direction of the displacement of atoms within the wave. During the course of a normal vibration all the atoms of the crystal vibrate harmonically near their equilibrium positions at the same frequency ω which is determined by the dispersion law that connects the values of ω and k: ω2 = fα (k),

α = 1, 2, . . . , 3q,

where α denotes the branch of the dispersion law and q is the number of atoms in the crystallographic unit cell. In three dimensions there are at least three branches of vibrations. In the long-wave approximation (λ a, a is the interatomic distance) all the atoms in the unit cell vibrate with the same phase, corresponding to acoustic vibrations (Fig. 1(a)). In this limit λ a they are transformed into the usual sound waves in a solid with the linear dispersion law ω = cs k, s = 1, 2, 3. Acoustic vibrations cover the frequency band from 0 to 1013 Hz. At high frequencies the dispersion law is no longer linear. However, in the

CRYSTAL LATTICE DYNAMICS

245

Fig. 1. Diagram of a long-wave vibration of a one-dimensional crystal: (a) acoustic mode; (b) optical mode.

Debye model it is assumed that acoustic vibrations satisfy the linear dispersion law at all frequencies within the range 0 < ω < ωD , where the Debye frequency ωD is the maximum possible vibrational frequency (1013 Hz), and serves as the most important parameter of the spectrum of crystal vibrations. In a complex crystal lattice (q > 1), 3q − 3 branches of optical vibrations are possible, and at k = 0 the center of mass of the unit cell remains stationary with the motion reduced to relative displacements of atoms within the unit cell (Fig. 1(b)). In the limit k → 0 the optical vibration frequencies ω(0) are different from zero. Ordinarily the frequency bands of optical vibrations are located above those of acoustic vibrations, with a forbidden region, or band gap, separating them. It is also possible for acoustic and optical frequency bands to overlap. There are crystals in which some optical frequencies strongly depend on external parameters (temperature, pressure, magnetic ﬁeld, etc.) and at speciﬁc values of these parameters they may tend to zero (soft modes). As a result, static relative displacements of atoms can occur, i.e. the unit cell is restructured by undergoing a structural phase transition. Optical vibrations of ionic crystals can strongly interact with an electromagnetic ﬁeld producing coupled polarized vibrations of the lattice and the ﬁeld. This phenomenon permits the excitation of optical vibrations of ionic crystals by incident oscillating electromagnetic ﬁelds (e.g., light waves), generally in the IR frequency range, which is the reason for calling these frequencies optical.

Many lattice modes can be excited simultaneously with different amplitudes. The total number of possible independent vibrations equals the number of mechanical degrees of freedom of all the atoms in the crystal, and their distribution in frequency is determined by the frequency distribution function ν(ω) (phonon density of states). The form of ν(ω) strongly depends on the dimensionality of the crystal. In a three-dimensional lattice at low frequencies (ω ωD ) for each acoustic branch ν3 (ω) ∝ ω2 /ωD 3 . For increasing frequency the behavior of ν(ω) changes: it tends to zero at the band edges, and within the bands it exhibits Van Hove singularities (Fig. 2). The overall vibrational density of states is obtained by summing the distributions of the individual branches. The quantum dynamics of a crystal lattice is well described by the harmonic approximation: to each wave of normal vibration with frequency ω and wave vector k there is a corresponding quasi-particle with the energy ε = ω and quasi-momentum p = k, with the number of quasi-particles proportional to the wave intensity. These quasi-particles are the elementary excitations of crystals and are called phonons; they obey Bose–Einstein statistics and form an ideal gas in the harmonic approximation. At sufﬁciently low temperatures when the crystal is weakly excited mechanically, its thermodynamic properties arise from these elementary excitations, and in particular the lattice portion of the crystal energy coincides with energy of the phonon gas. The quantum nature of the crystal motions is manifested through the presence of so-called

246

CRYSTAL LATTICE VIBRATIONS

(1)

Fig. 2. Plot of the frequency distribution function in a three-dimensional crystal for the acoustic (0 < ω < ωm ) and (2) (3) optical (ωm < ω < ωm ) branches, where ω1 , ω2 , ω3 , ω4 are the frequencies of Van Hove singularities.

zero-point vibrations of atoms at T = 0 K. The amplitude of these vibrations is usually considerably smaller than the interatomic distance, but in crystals consisting of light atoms it may not be so very much smaller (quantum crystals He, H2 , Ar). In solid He the zero-point vibrations are so pronounced that the solid state exists at T = 0 K only under a pressure of more than 25 atm. At lower pressures it “melts” and transforms into a quantum liquid. Other crystals simply melt with an increase in temperature. Melting involves the disruption of the crystal structure and the long-range order, and it occurs when the average amplitude of vibrations of atoms exceeds some critical value. With increasing amplitudes of vibration, anharmonic behavior begins to appear. Anharmonic vibrations cause interactions of phonons and play an important role in kinetic processes such as thermal conductivity and sound absorption in crystals. The interaction of phonons with other elementary excitations (electrons, excitons, spin waves) inﬂuences the dynamics of the crystal lattice through the electrical conductivity, and the optical and relaxational properties of the crystals. The dynamic interaction of a crystal with photons (including X-rays and γ -quanta), neutrons and accelerated charged particles not only reﬂects the structural features of the crystalline state, but also provides experimental methods for investigating the dynamics of crystal lattices. For example, inelastic neutron scattering can furnish the dispersion law and polarization of the vibrations; and the Mössbauer effect can provide estimates of the rootmean-square displacements of vibrating atoms.

CRYSTAL LATTICE VIBRATIONS

Coherent oscillatory motion associated with a crystal lattice. The theory of crystal lattice vi-

brations uses the Born–Oppenheimer adiabatic approximation (M. Born and R. Oppenheimer, 1927), whereby the relatively light and fast moving electrons adiabatically follow the relatively slow motion of heavy atomic nuclei or ions. This justiﬁes presenting the potential energy of a crystal as a function of atomic coordinates only. Assuming small vibrational amplitudes, the potential energy is expanded in a power series in the displacements of atoms from their equilibrium positions. Taking into account only quadratic terms of the expansion corresponds to the harmonic approximation, and leads to linear equations of motion. If us (n) is the displacement of the sth atom in the unit cell of vector-number n, its variation with time is given by the equation: ms d2 uls (n) ik + βss (n, n )uks (n ) = 0, dt 2 nsk

where ms is the mass of the sth type of atom, i and ik (n, n ) are force k are Cartesian indices, and βss constants. Normal vibrations emerge as eigensolutions of the lattice vibration equations. There are 3 acoustic vibration modes and 3q − 9 optical vibration modes for q > 3 (q is the number of atoms in the crystallographic unit cell). Thus the superconductor Tl2 Ba2 CaCu2 O8 has 3 acoustic modes and 36 optical modes of vibrations (16 Raman active and 20 infrared active). CRYSTALLINE STATE, GASEOUS See Gaseous crystalline state.

CRYSTALLIZATION

CRYSTALLITE, MICROSee Microcrystallites. CRYSTALLITES

Small crystal grains (see Polycrystal) in various polycrystalline formations: metal ingots, processed metals and alloys, rocks, minerals, ceramics. Fine monocrystals lacking a clear crystallographic polyhedral shape, and large microcrystals with poorly developed structure (dendrites), plastic deformed microcrystals, etc., are also called crystallites. Depending on the nature and conditions of formation, the average size of crystallites varies within the limits 5–10 μm, with their orientation either arbitrary or following certain patterns (textures). As far as their shape is concerned, crystallites may be equiaxial, columnar, platelike, etc. The crystallite structure strongly affects the strength, plasticity, and other properties of a substance as a whole. Quenching the liquid phase yields particularly ﬁne crystallites, down to the so-called X-ray amorphous structure range (crystallites below 3 nm in size). CRYSTALLIZATION

The process of transforming a substance from its liquid, amorphous or gaseous phase into a crystal. For a crystal to form it is necessary for the chemical potential μ of the crystal phase (which depends on pressure p, temperature T , and concentration c) to be lower than the respective chemical potential of the initial phase. Since a crystal phase usually corresponds to lower temperatures, higher pressures and concentrations in the phase diagram than those found at the point of phase equilibrium, one needs to produce overcooling T , excess pressure p, or supersaturation

c in the initial phase. The relation between

T , p, c and the change in chemical potential, μ, may be expressed as

T , T

p

μ = kB T , p

μ = H

(1)

c , c where H is the change in enthalpy per particle during the phase transition, and k B is the Boltzmann constant.

μ = kB T

247

Crystallization may occur via random formation and growth of crystal precipates (embryos) in various parts of the total volume of the initial phase, a process called mass crystallization. During the formation of a precipitate the binding energy of particles entering it (either atoms or molecules) is released. Energy is expended to form the precipitate surface. For a spherical precipitate of radius r the total change of thermodynamic potential is w(r) = −

4π 3 μ r + 4πr 2 α, 3 v

(2)

where v is the volume per individual atom or molecule, and α is the interphase energy per unit surface area of the precipitate (coefﬁcient of surface tension). The function w(r) is nonmonotonic, and reaches a maximum at r = 2αv/ μ. The corresponding radius of the precipitate is called the critical radius r c , and the energy of its formation is w(rc ) = (16π/3)(α 3 v 2 / μ2 ). Precipitates of a critical radius (see Critical embryos) are in a state of unstable equilibrium with their environment. An increase or decrease of the precipitate radius results in its growth or decay, respectively. When a precipitate forms in an initial phase containing no extraneous microimpurities, the process of its formation is called homogeneous precipitation. When the initial phase contains microimpurities, critical precipitates may form at their surface (or on the walls of the container). In that case, the formation process is called heterogeneous precipitation. The ratio between the work required to form precipitates of a critical radius heterogeneously and homogeneously is given by 1 ψ(θ) = (1 − cos θ)2 (2 + cos θ), 4

(3)

where θ is the edge angle depending on the coefﬁcient of surface tension at the system interfaces. These are the initial phase–microimpurity; microimpurity–crystal; and crystal–initial phase interfaces. Wetting lowers the work of precipitate formation. The number of precipitates of a critical radius per unit volume of the initial phase is proportional to the probability of their formation: exp[−w(rc )/(k B T )]. The respective proportionality coefﬁcient is close to the number of molecules

248

CRYSTALLIZATION CENTER

in a unit volume, n. The rate of formation of precipitates I , i.e. the number of precipitates formed in a unit volume per unit time, may be determined within the formalism of the thermodynamic theory of their formation. One has to multiply the density of precipitates of a critical radius by the number of atoms (molecules) striking their surface per unit time: ⎧ 4πrc2 pn(2πmk B T )−1/2 , ⎪ ⎪ ⎪ ⎪ ⎨ precipitatesform from gas phase, E I= 2 , 4πrc nνa exp − ⎪ ⎪ ⎪ kBT ⎪ ⎩ precipitates form from condensed phase, where m is the mass of the molecule, a is the atomto-atom distance, ν is the frequency of atomic oscillations, and E is the activation energy for particles adding to the precipitate. To account for the evolution of the system of precipitates of radii below rc in the initial phase one adds an extra term in the expression for I , namely: 4rc α 1/2 , z= 9k B T nc where nc is the number of particles in a precipitate of a critical radius. With decreasing temperature (at relatively small overcooling) I grows as precipitates grow, since their formation energy diminishes; on the other hand, the energy of thermal motion and the mobility of particles in the initial phase simultaneously decrease, so that the rate at which they add to the surface of the precipitate decreases as well. Competition between these two factors produces a maximum of I at a certain temperature, after which it starts to decrease at lower temperatures. The value of I is remains negligibly small at comparatively small supercooling (or supersaturating) of the initial phase, so that very few precipitates form in volumes of appreciable size. In other words, the initial phase remains in a metastable state. The range of respective supercooling (supersaturating) is called the metastability range. As a result of the mass crystallization a polycrystal forms, with ﬁne crystals growing from separate precipitates (crystallites) that ﬁll the volume of the initial phase with their crystallographic axes randomly oriented. The structure of the polycrystal depends on the values of I and v. Its

granularity roughens for larger I and smaller v. See also Monocrystal growth. CRYSTALLIZATION CENTER See Crystal nuclei. CRYSTALLIZATION FROM THE GAS (VAPOR) PHASE The formation of crystals by the transformation

of a material from its gas (vapor) phase to a solid. When crystals grow from the vapor an adsorption layer differing from the crystal in composition and properties appears at the crystal–medium interface (see Adsorption). Moreover, surface diffusion of the adsorbed particles at the growing faces plays a decisive role there. Crystallization from the gas phase has been used to produce massive monocrystals, plates, bands, acicular crystals, thread-like crystals, and epitaxial lm s. Condensation techniques and chemical reactions are also employed to grow crystals. When using the ﬁrst it is assumed that material reaches the growing crystal as an atomic or molecular vapor, or as associations of such particles. Depending on the technique used to bring the material to the crystallization zone one may speak about molecular beams in vacuo (see Molecular beam epitaxy), cathode sputtering (see Sputtering), volume vapor phase in an isolated system, and crystallization in an inertial gas ﬂow. To obtain high quality crystals and ﬁlms chemical reaction techniques (e.g., as chemical transport, decomposition of compounds, chemical synthesis in the vapor phase) appear to be quite efﬁcient. In certain cases when ﬁlaments or massive crystals are grown (as well as epitaxial ﬁlms), the vapor–liquid–crystal transport mechanism is employed. Vapor material reaches the growing crystal through a liquid layer of different composition formed either unintentionally or intentionally on the growing surface by introducing impurities into the crystallization zone. It may result from deviations from a stoichiometric composition, or present a liquid phase intentionally formed at the substrate as a smelt droplet of a prescribed composition. The phase-to-phase energy of the crystal–vapor interface is almost an order of magnitude less than the respective energy of the crystal–vapor interface. Two-dimensional precipitates (embryos)

CRYSTALLOGRAPHIC INDICES

form at the liquid–crystal interface at a rate that is much higher than such a rate at the vapor–crystal interface. This feature combines with other factors (such as a higher condensation coefﬁcient at the liquid surface, low resistance to diffusion in the smelted droplets, etc.) to sharply increase the growth rates. CRYSTALLIZATION, HYDROTHERMAL See Hydrothermal crystallization. CRYSTALLIZATION OF POLYMERS First-order phase transition in polymeric systems. Crystallization of high molecular weight

polymers is more complex than crystallization of low molecular weight substances because of the inﬂuences of various parts of the polymer chains (main chain links and side branches). Long chain polymers have a primary structure from the linking together of their repeat units or monomers. A secondary structure can arise from coiling or linking nearby parts through weaker hydrogen bonds, and a tertiary structure can form if larger sections fold into themselves to form a globular or condensed conformation. A crystal structure can form from stretched out and aligned macromolecular chains, from regularly arranged molecular chains folded “upon themselves”, from adjacent polymers interlinked in a quaternary structure, etc. These various conformations of the macromolecule as a whole are found in a crystal with unchanged sublattice parameters (repeatedly packed chain links or monomers), and an unchanged translation period along the primary chain axis. There are globular crystals, supercrystals, with long-range ordering in the packing of the macromolecules (see Long-range and short-range order), e.g., globular proteins or their elements (blocks, co-polar blocks). Such longer range ordering may be present along with short range ordering in the packing of repeated molecular chain links. Deformation processes affecting the conformations of macromolecules can affect the ability of some polymers to crystallize (polyisobutylene is an example). CRYSTALLIZATION, SELF-SUSTAINING See Self-sustaining crystallization.

249

CRYSTALLIZATION WAVES

A particular form of slowly damping oscillations of the interface between solid and liquid helium at low temperatures (below the lambda point 2.17 K) where liquid 4 He is a superﬂuid quantum liquid (see Super uidity) and solid 4 He is a quantum crystal. When a crystallization wave propagates through this system it is accompanied by periodically alternating melting and crystallization. When crystallization waves are mechanically excited, the surface of a 4 He crystal goes into a dynamic state of quantum roughness, similar to a thermodynamic equilibrium state of atomic roughness found at the surface of a classical crystal (see Phase transitions at a surface). The spectrum of crystallization waves at low frequencies has the form: ρL k 3 ρL k +g ρS − ρL (ρS − ρL )2 ρL ρS − iωk , K(ρS − ρL )

ω2 = α

where ω and k are the frequency and the wave number of the crystallization waves; ρ L and ρ S are the densities of the liquid and the solid, respectively; g is the free fall acceleration (9.8 m/s2 ); K is the kinetic coefﬁcient of growth (proportionality coefﬁcient between rate of growth of a rough crystal face, and difference between crystal and liquid chemical potentials); α = α + ∂ 2 α/∂ϕ 2 is the surface rigidity of a given face of the crystal (α is the speciﬁc surface energy, and ϕ is the crystallographic angle corresponding to the direction k). The value of K for helium is particularly large below 0.7 K so propagating crystallization waves are only weakly damped. CRYSTALLOGRAPHIC CLASSES The same as Crystal classes. CRYSTALLOGRAPHIC INDICES

A triplet (quadruplet) of numbers deﬁning the position of points (sites), directions and planes in a lattice. Let the radius-vector from the origin to a given site in the crystal lattice be projected on to the a, b, c axes in a (in general, oblique) coordinate system so that these projections are equal to ax, by, cz. Then x, y, z are the crystallographic indices of that site, and the direction of

250

CRYSTALLOGRAPHIC SYSTEM Table 1. Crystallographic classiﬁcation scheme System

Triclinic (anorthic) Monoclinic Orthorhombic Trigonal Hexagonal Tetragonal Cubic (isometric)

Number of

Example of point group

space groups

International

Schönﬂies

2 13 59 25 27 68 36

1 2/m mmm 3m 6/mmm 4/mmm m3m

Ci C2h D2h D3d D6h D4h Oh

a vector to that site is denoted by [xyz]. A vector parallel to the x coordinate axis is in the [100] direction, etc. Crystallographic planes are denoted by what are called Miller indices (hkl). Consider a plane which intersects the a, b, c axes at the points h a, k b, l c, and write down the reciprocals of these intercepts 1/ h , 1/k , 1/ l . The Miller indices are the smallest three integers h, k, l having these same ratios. For example, if h = 4, k = 1 and l = 2 then (hkl) = (142). The three integers which deﬁne orientation directions in a crystal, and the positions of its verges, are called the Weiss indices, and they are written in the form [p1 p2 p3 ]. As for the hexagonal system and the trigonal system, their directions and planes are sometimes presented in a four axes system (three equivalent directions are then positioned at 120◦ to each other in the basal plane of the crystal). The Bravais indices [mnrp] and (hkil) satisfy the conditions r = −(m + n), i = −(h + k). When using the Bravais indices one may clearly see the equivalence of the respective directions and planes in the crystal. CRYSTALLOGRAPHIC SYSTEM

Crystallographic classiﬁcation scheme for the 230 space groups that takes into account their characteristic symmetries (see Crystal symmetry), and uses the ratios of their symmetry axes. There exist seven independent combinations of the rotation symmetry axes of the nth order (n = 1, 2, 3, 4, 6), and seven crystallographic systems corresponding to them: cubic system, hexagonal system, trigonal system, tetragonal system, orthorhombic system, monoclinic system and triclinic system. The concept of crystallographic system

coincides with the concept of syngony for every crystallographic system, with the exception of the hexagonal and the trigonal systems which together comprise the hexagonal syngony or family. Table 1 outlines the crystallographic classiﬁcation scheme, and lists a high-symmetry point group for each system. CRYSTALLOGRAPHIC TEXTURE See Texture. CRYSTALLOGRAPHY (fr. crystal, and Gr. γραϕω, am writing) The science describing crystals and the crys-

talline state of matter. Six basic branches are recognized within crystallography: geometric crystallography (crystal symmetry, crystal structures, and crystal morphology); crystallogenesis (crystal formation and growth, see Crystallization); crystal physics; crystal chemistry; applied crystallography (methods and techniques for crystal growth and use in technical applications); space crystallography or growing crystals in zero gravity (in orbit) and studying their properties. Geometric crystallography gave birth to the hypothesis of ordered three dimensional positioning of particles (atoms and molecules) composing the crystal which form the crystal lattice. The mathematical apparatus of crystallography is based on Euclidean geometry, group theory, and tensor calculus. Structural crystallography studies the atomic and molecular composition of crystals using X-ray structure analysis, electron diffraction analysis, and neutron diffractometry, all based on the diffraction of waves and particles within the crystals. Optical spectroscopy, electron microscopy, and

CRYSTAL MORPHOLOGY

resonance methods, etc., are sometimes used. As a result, the crystal structures of over a hundred thousand chemical substances have been determined. When studying the processes of formation and growth of crystals one uses the basic principles of thermodynamics, the laws of r st-order phase transitions, and of surface phenomena. One also accounts for the interaction of crystals with their ambient environment, and for anisotropies. Industrial processes used to grow diamonds, rubies, and other crystals have been perfected (see Synthetic monocrystals), and provide a basis for quantum and semiconductor electronics, optics, acoustics, etc. Crystallography also studies various perturbations in an ideal crystal lattice, such as defects and dislocations, that originate during the course of crystal growth due to various external inﬂuences, and inﬂuence many properties of crystals. The structure and properties of various aggregates formed from microcrystals (polycrystals, textures, ceramics), as well as substances with atomic ordering similar to that found in crystals (liquid crystals, polymers), are also studied. Consistent symmetrical and structural patterns studied within the framework of crystallography ﬁnd their application when treating general structural features and properties of various non-crystalline states of condensed matter, such as amorphous solids and liquids, polymers, macromolecules, supermolecular structures, etc. (generalized crystallography). Studies of biological crystals have been successful in determining the structures of large protein and nucleic acid molecules. Modern crystallography typically concentrates on the atomic and defect structure of crystals, processes of their formation and growth, and searches for new properties of crystals. These problems involve comprehensive tasks aiming at discovering new materials with important physical properties. Results obtained from crystallographic studies are routinely applied to physics, mineralogy, chemistry, molecular biology, etc.

CRYSTAL MORPHOLOGY (fr. Gr. μoρϕη , appearance, shape, and λoγ oς , word) Outward shape of crystal that grows from a

solid, liquid or gaseous phase. It depends on the nature of the substance, on growth conditions, and other factors. During crystallization from the melt with a small deviation from equilibrium, crystals of some materials grow in the shape of regular crystal polyhedra (Fig. 1), while crystals of other materials grow in a shape approximating a sphere (Fig. 2(a)). A faceted shape (see Crystal faceting) is typical of materials that exhibit a high entropy of fusion S = L/T > 4R (L is the latent heat of melting, R is the gas constant), and a high anisotropy of surface energy. A rounded shape is typical of metals and other materials that exhibit a low entropy of fusion ( S < 4R) and a low surface energy anisotropy. Metals grown from a gaseous phase or from solution may exhibit a faceted shape. A smooth shape loses stability and develops bulges (Fig. 2(b)) at increased overcooling of the melt (in metals, this process occurs at smaller values of overcooling, than in crystals with a high entropy of fusion). The presence of impurities intensiﬁes this process owing to emerging structural overcooling. Thermal and structural overcooling ﬁrst results in the formation of bulges (cellular morphology), which then evolve into dendrites (Fig. 2(c, d)). Under sufﬁciently high overcooling, the dendritic shape degenerates into a needle one without lateral branches. When crystallization takes place from a viscous medium,

CRYSTALLOGRAPHY, INTERNATIONAL TABLES See International Tables for Crystallography. CRYSTALLOGRAPHY, TWO-DIMENSIONAL See Two-dimensional crystallography.

251

Fig. 1. Crystal polyhedron.

252

CRYSTAL NUCLEI

Fig. 2. Crystal morphologies.

spherulites form, which are monocrystalline ﬁlaments or crystallite aggregates of radial-beam shape. CRYSTAL NUCLEI, crystallization centers

Crystal phase clusters of critical (and larger) sizes with the capability of growing (see Crystallization) in a melt. The critical size of a crystal nucleus is associated with the equality of the bulk and the surface parts of its free energy (which decreases as the melt is overcooled). Crystallization centers may appear spontaneously on solid surfaces, where this process is facilitated by the formation of crystal nuclei.

CRYSTAL OPTICS

The branch of optics investigating light propagation in crystals. Among phenomena of crystal optics, there are birefringence, interference and polarization of light, optical activity (see Rotation of light polarization plane), conical refraction of light, pleochroism, etc. These phenomena can appear or vary under the action of external electric and magnetic ﬁelds, mechanical stress, acoustic waves, and this is the subject of electron, magnetic, piezo-, and acoustic optics, respectively. The classical approach to the phenomena of crystal optics is based on the electrodynamics of continuous media, crystal symmetry, tensor cal-

CRYSTAL OPTICS

culus; it is based on the fact that the period of a crystal lattice (∼1 nm) is much shorter than the wavelength of light (∼500 nm), and therefore, a crystal can be considered as a homogeneous anisotropic medium. This is expressed by a tensor form of material equations connecting the electric ux density Di and magnetic ux density Bi with the corresponding ﬁelds Ej and Hj : Di = εij Ej and Bi = μij Hj (here εij and μij denote the polar tensors of rank two of dielectric constant and magnetic permeability). In most problems of crystal optics, one considers nonmagnetic crystals (μij = 1) and concentrates upon the properties of the tensor εij . In the absence of spatial dielectric dispersion, the dissipation of energy, and an external magnetic ﬁeld, by the symmetry principles of kinetic coefﬁcients, the tensor εij is symmetric and real. Therefore, for a ﬁxed frequency of light ω, in anisotropic media, the directions of vectors D and E do not coincide. This determines the anisotropy of the optical properties of crystals, i.e. the dependence of the phase veloc√ ity v = c/n and of refractive index n = ε on the direction. For the totality of all directions at an arbitrary point of a crystal, the magnitudes of n form an ellipsoidal surface, which is called the optical indicatrix. The symmetry axes of the optical indicatrix form three mutually orthogonal principal directions in the crystal (crystallophysical axes), along which the directions of vectors D and E coincide. In the rectangular Cartesian coordinate system with axes coinciding with the crystallophysical axes, the equation of the optical indicatrix is of the form x2 n2x

y2 z2 + 2 + 2 = 1, ny nz

where nx , ny , and nz are the principal values of n. Crystals of a cubic system are optically isotropic, i.e. their ellipsoid degenerates into a sphere; the crystals of medium systems are optically uniaxial (the indicatrix is an ellipsoid of revolution); the crystals of lower systems are optically biaxial (the indicatrix is a triaxial ellipsoid). The optical axis of a crystal corresponds to the normal of a circular section of the optical indicatrix. The laws of propagation of plane harmonic waves in dielectric crystals follow from the wave

253

equation together with the tensorial relation between the vectors D and E. Thus, we get the dispersion equation, which corresponds to a homogeneous system of three linear equations for the components of the vector E: εij (ω)ω2 2 δ + k k E (ω) = 0, − k ij i j j c2 where k, ki , and kj are the magnitudes of the wave vector and its corresponding components, δij = 0 for i = j , and δij = 1 for i = j . This system has a nontrivial solution E = 0 if and only if the determinant in the parentheses is not zero. The latter condition leads to the Fresnel equation ky2 kz2 + + = 0, v 2 − vx2 v 2 − vy2 v 2 − vz2 kx2

where v is the magnitude of the phase velocity, the direction of which coincides with the direction of the wave vector k; vx , vy , and vz are the principal phase velocities of the wave for the corresponding directions of the vector D when the light propagates along one of the principal directions. The dispersion and Fresnel equations are quadratic with respect to k and v, i.e. at light propagation in anisotropic crystals, there arise two waves (see Fig.) with different values of the magnitude of the wave vector and different phase velocities (refractive indices) v1 and v2 coincide only along the directions of the optical axes. They correspond to two mutually orthogonal values of the vectors D and E. If from some point of the crystal one locates all the vectors corresponding to v1 and v2 in all the directions m, then the endpoints of these vectors form two surfaces called the surfaces of normals. In uniaxial crystals, one of these surfaces is a sphere (characterizing the ordinary ray v0 ), and the other one is an ellipsoid of revolution (characterizing the extraordinary ray ve ) tangent to the sphere at its intersection points with the optical axis. In biaxial crystals, both surfaces are ellipsoids intersecting at 4 points lying pairwise on two optical axes (binormals). The ray vectors form similar surfaces called ray surfaces (or wave surfaces). Thus, in anisotropic crystals, in an arbitrary direction m, there may propagate two plane waves polarized in two mutually orthogonal planes. The

254

CRYSTAL, PERFECT

Crystal optics.

directions of vectors D 1 and D 2 of these waves coincide with axes of the ellipse of the central section of the optical indicatrix by the plane orthogonal to m, and the lengths of the ellipse axes determine their refractive indices. Consequently, the optical indicatrix and surfaces of normals are mutually dependent. The birefringence in the crystals because of the different refraction indices of two polarized waves propagating in the same direction implies a path difference. If, in a convergent light, one reduces the polarization of these waves into one plane (using some polarization devices), this results in the interference of the light. Such interfering conoscopic images allow one to investigate crystal-optical properties of crystals. In the presence of a spatial dispersion of ﬁrst order with respect to k or an external magnetic ﬁeld, and also in magnetic crystals, the tensor εij is complex and, in general, nonsymmetric; moreover, εij (ω, k, H ) = εij (ω, −k, −H ). In particular, in such crystals two elliptically polarized waves propagate with orthogonal axes of the ellipse coinciding with the axes of the section ellipse of the optical indicatrix. The directions of by-pass of vectors E are opposite in both waves. Along the direction of the optical axis, and in cubic crystals, the polarization ellipses degenerate into circles, i.e. the waves are circularly polarized and have

different velocities. Moreover, in uniaxial crystals, the surfaces of normals do not osculate at the points of intersection with the optical axis. The ellipticity of waves brings about optical activity of crystals, which is expressed, e.g., as gyration, electrogyration, Faraday effect, etc. The complexity of the tensor εij and the elliptical two-ray refraction are also caused by light absorption in crystals. The directions of by-pass of ellipses in this case coincide. In such crystals, the absorption of differently polarized waves is different, and occasionally circular dichroism takes place in optically active crystals. Crystal optics adjoins crystallography, solid state physics, and mineralogy. With the appearance of laser technology, new branches of physical optics and optical tool making arose that are fundamentally based on crystal optics: coherent and nonlinear optics, holography, optoelectronics, integrated optics, etc. The control of optical (in particular, laser) radiation is based on the phenomena of crystal optics. CRYSTAL, PERFECT See Perfect crystal, Ideal crystal. CRYSTAL PHYSICS, physical crystallography Branch of crystallography involving the physical properties of crystals and crystalline aggregates of polycrystals, as well as changes in their

CRYSTAL PHYSICS

properties arising from external inﬂuences. Crystal physics explains anisotropy of crystals, and basic variations in the properties of crystals due to the regular distribution of particles (molecules, atoms, and ions) in the crystal lattice, and the types of their interrelations. The mathematical apparatus of matrix algebra, tensor calculus, and group theory provides a quantitative description of the physical properties of crystals. Directionally independent properties such as density are characterized by scalar variables. To describe physical properties involving relationships between two vectors (e.g., between either polarization or electric current density and electric ﬁelds, etc.) or between pseudo-vectors (e.g., magnetic induction and magnetic ﬁeld strength) one uses second-rank tensors (e.g., dielectric constant and magnetic permeability tensors). Many physical ﬁelds in crystals (e.g., electric and magnetic ﬁelds, mechanical strains) are themselves tensor ﬁelds. The relation between the physical ﬁelds and the properties of crystals may be described by tensors of higher rank, as is the case with the piezoelectric effect (see Piezoelectricity), electrostriction, magnetostriction, elasticity, photoelastic tensor, etc. It is convenient to represent dielectric, magnetic, elastic, and other physical properties of crystals in the form of characteristic surfaces such as ellipsoids. The radius-vector that traces out such a surface indicates the value of a particular property along its given direction (see Crystallographic indices). The symmetry of any property of a crystal may not be lower than the symmetry of its external shape (Neumann principle, F. Neumann). In other words, a symmetry group G1 that describes any physical property of a crystal includes necessarily the symmetry elements of its associated point group G, that serves as its supergroup: G1 ⊃ G. The symmetry elements determine the orientations of the principal axes of characteristic surfaces, as well as the number of tensor components that determine a given physical property. In many cases these are surfaces of ellipsoids with their principal axes related to the symmetry axes of the crystal (see Crystal classes). Crystals of low symmetry have their physical properties described by second-rank tensors with three principal values (plus the orientation of the tensor principal axes). Physical properties of cubic symmetry crystals that are described by second-rank tensors are

255

directionally independent or isotropic. Crystals of intermediate symmetry (tetragonal, trigonal and hexagonal) have these properties characterized by the symmetry of their rotation ellipsoid, i.e. their second-rank tensors have two independent components, one of which describes the property along the principal axis, and the other along any direction orthogonal to this axis. To describe the property along an arbitrary direction one needs to know these two principal components plus the direction cosines of the direction. Physical properties described by higher-rank tensors are characterized by a larger number of parameters: e.g., elasticity properties, described by a fourth-rank tensor, need three such variables in a cubic crystal, and two independent variables in an isotropic medium. The elastic properties of a triclinic crystal require 21 independent tensor components for their description. To determine the number of independent components of tensors of higher rank (5th, 6th, etc.) one can make use of the corresponding point group of symmetry. To obtain a complete description of the physical properties of crystals and textures one may make use of radiofrequency, acoustical, optical, and other techniques. Crystal physics studies both phenomena speciﬁc for anisotropic media (birefringence, rotation of light polarization plane, direct and inverse piezoeffects, electro-optic, magneto-optic, and piezooptic effects, generation of optical harmonics, etc.), as well as properties more often associated with isotropic media (electric conductivity, elasticity, etc.). In crystals these latter properties may also exhibit features resulting from the crystal anisotropy. Many phenomena within the scope of crystal physics are related to changes in the crystal symmetry under various thermodynamic conditions. The Curie principle may be used to predict changes in both the point and the space symmetry groups of crystals undergoing phase transitions, e.g., entering ferromagnetic or ferroelectric states (see Ferromagnetism, Ferroelectricity). Crystal physics studies various defects of the crystal lattice (color centers, vacancies, dislocations, grain boundaries, stacking faults, domains, etc.) and their effects upon the physical properties of crystals (plasticity, strength, luminescence,

256

CRYSTAL POLYHEDRON

electrical conductivity, mechanical Q-factor, etc.). Among the tasks of crystal physics is the search for new crystalline materials with speciﬁc prospective properties needed for practical technological applications. CRYSTAL POLYHEDRON A monocrystal grain under equilibrium conditions (see Monocrystal growth) consisting of a

certain combination of faces, edges and vertices. The number of faces, edges and vertices should follow the Euler theorem (L. Euler): the sum of the number of faces and vertices equals the number of edges plus two (F + V = E + 2). The socalled simple forms participate in crystal faceting. These are polyhedra whose faces can be obtained from one another via symmetry operations that are speciﬁc for the crystal class of the given crystal; they usually form various combinations with each other. There are 47 geometrically distinct simple forms known; this number increases to 193 when taking into account enantiomorphous (mirror reﬂection) pairs (see Enantiomorphism), or to 146 in case one accounts for differences in point symmetry. Only certain simple forms are permissible in each point group. Speciﬁc forms of crystal polyhedra depend on their structure and conditions of crystallization. CRYSTAL, QUANTUM See Quantum crystals. CRYSTALS (fr. Gr. κρυσ τ αλλoς , ice) Solids with ordered three-dimensional periodic

spatial atomic structure. The formation medium may be an overcooled vapor or liquid of a pure substance, a supersaturated solution or ﬂux of one material in another (the solvent), or a crystal medium of a polymorphous modiﬁcation or composition different from that of the newly formed crystal. Some features of crystals depend on their formation process. If the material is supplied evenly and uniformly from the ambient environment then a polyhedral shape results, limited by ﬂat faces intersecting each other along straight edges. These faces, often mirror smooth in perfect crystals, are tilted toward each other at certain angles characteristic for the particular crystal type (law of constancy of angles). The ratios between

the intercepts on the axes for different tilted faces of a crystal can always be expressed by rational numbers such as 1 : 2 √ or 2 : 3, and never by irrational ones such as 1 : 2 (law of rational indices). Other general macroscopic properties of crystalline matter include crystal homogeneity (independence of the choice of measurement point), anisotropy of crystals (dependence on direction), and crystal symmetry (spatial transformations that bring the crystal into itself). There are 32 classes of morphological symmetry of crystals, each corresponding to its speciﬁc set of symmetry elements: axes, planes, center of symmetry, etc. Three-dimensional atomic structure periodicities are described in terms of a threedimensional space lattice (the crystal lattice), a three-dimensional periodic system of points that may be formed starting from an arbitrary point by simply repeating the lattice by a series of parallel translations. There exist a total of 14 types of such lattices called Bravais lattices. The crystal appearance (crystal morphology) is characterized by the crystal shape and faceting, i.e. the set of faces bounding the crystal, and by the ratio of the sizes of these faces (see crystal faceting). Such facets and their relative sizes characterize the crystal morphology or crystal habit. The shapes of crystals reﬂect their crystal structure, and the nature of the interactions between their atoms. In particular, these factors affect the shape of the forming crystal through kinetic phenomena occurring at the surface of a growing crystal. Such phenomena depend on the level of supersaturation, temperature, composition of the ambient medium, thermal conductivity, diffusion, and the presence of impurities. The shape acquired by the crystal during its growth (the growth shape) is very sensitive to the conditions of crystallization, and reﬂects the mechanism of growth. Therefore, the growth shape implies certain conclusions beyond the conditions of growth. During the artiﬁcial growth of crystals the crystallization parameters may be chosen accordingly. Although a typical crystal shape is a polyhedron, rounded growth shapes or strongly perturbed shapes may form under certain ambient conditions (thread-like crystals, plates, dendrites, etc.). Some crystals can form in two different modiﬁcations, a right-hand and left-hand one (enantiomorphism). Substances

CRYSTAL STABILITY CONDITIONS

are found that may crystallize in the shape of twins (twinning of crystals). In cases when crystal faceting is suppressed by the limited availability of feeding material, forced growth shapes develop. The crystal can then acquire the shape of the surface limiting its growth (e.g., crucible walls, smelting isotherm in a smelt, an isoconcentration saturation surface in a gas phase). Most monocrystals are the result of forced growth. Technologies for growing crystals with forced growth shapes ﬁnd wider and wider applications. Almost all semiconductor crystals are produced that way, as well as most piezoelectric, ferroelectric, and optical crystals (see Monocrystal growth). If crystal generation and growth occur simultaneously throughout the whole volume a polycrystal forms, that is an aggregate of randomly oriented ﬁne crystals of various sizes and shapes called crystallites or crystal grains. Sometimes crystallites follow a certain predominant orientation indicating the presence of a texture. During mass crystallization when embryos appear only in certain regions of the generating medium, the collective growth of crystals ensues, characterized by the interaction of the growing crystals with each other, to produce a geometric selection. Crystals having an optimal orientation for the given ambient conditions then survive. Such a competition results in the formation of a pole structure, typical for metal ingots, in which all the crystals are elongated and almost parallel to each other. Examples of such collective growth are druses (crystal agglomerations in which the vertices of separate crystals face in more or less the same direction) and parallel inshoots (crystals growing together to merge in a parallel orientation). The ideal structure of a crystal always undergoes certain perturbations (accumulates defects) because growth conditions change, impurities are trapped, and various external inﬂuences are always at work. Real crystals often display macrodefects (gas–liquid, solid inclusions, cracks, etc.) which worsen their properties. A typical structural defect is mosaicity (see Mosaic crystals) which results from various defects (internal stress, block boundaries, twins (see Twinning of crystals), stacking faults, dislocations, etc.) that appear during crystal growth. The presence of foreign atoms and ions (impurities) in a crystal during its growth may result in the development of zonal, sectional, and

257

other structures. Substituting crystal atoms (substitutional impurities) or imploding between the atoms of the crystal (implosion impurities) can produce point defects (see Impurity atoms). Other point defects perturbing the lattice periodicity are vacancies and interstitial atoms. The level of deﬁciency of the crystal structure affects both crystal growth (e.g., the dislocation mechanism of growth) and various crystal properties that are structure sensitive (plasticity, strength, electrical conductivity, photoconductivity, light absorption capacity, etc.). Therefore, to grow crystals with prescribed properties, one must intentionally introduce desired defect structures. Examples are donor and acceptor impurities which determine the electrical properties of semiconductors. Added impurities (doping) are widely used to produce semiconducting crystals with various types and levels of conductivity, to produce laser crystals with a prescribed spectral transmission band, etc. The development of electronics, quantum electronics, computer technology, and various other industries is directly linked to using crystals and complex crystal structures based on them (e.g., epitaxial layers, heterostructures, microchips, superlattices). CRYSTAL STABILITY CONDITIONS

Conditions imposed on the coefﬁcients of the expansion of the crystal potential energy U in terms of atomic displacements usi : U = U0 + Asi usi s,i

+

1 Ast ij usi utj + · · · , 2 s,t,i,j

where U0 is the crystal energy at equilibrium (the indices s and t are used for labeling atoms; i, j = x, y, z). From the condition that the resultant of all forces acting on the atoms at equilibrium vanishes, it follows that Asl = 0. From the inrotation of variance of U under translation and the crystal as a whole it follows that t Ast ij = 0, t (Ast ij Xt k − Ast ik Xtj ) = 0 (Xsi designates the sth atom coordinates). Crystal symmetry properties impose additional restrictions on the harmonic force constants Ast ij , and the application of these relationships considerably reduces

258

CRYSTAL STRUCTURE

the number of independent force constants. Besides that, some restrictions on the force constants follow from the condition of crystal equilibrium (U = min at equilibrium), and these are in the form of inequalities arising from the requirement of positive deﬁniteness for the quadratic form (third term) of the expansion of U . Similar conditions may be derived for the anharmonic force constants, which serve as the coefﬁcients of additional terms of the expansion of U . CRYSTAL STRUCTURE

The structure of an actual crystalline solid. The concept of crystal structure starts with the concept of crystal lattice, i.e. of the parameters of a unit cell, such that any ideal crystal (monocrystal) may be reproduced by repeating its unit cell in space. A full description of a crystal structure also includes specifying the positions of atoms, ions and molecules inside the cell (including the orientations of molecules). Beside the locations of the atoms, other important factors are the distribution of the electron density in the unit cell, the atomic and ionic radii, chemical bonds (see Crystal chemistry), coordination numbers (see Coordination sphere), etc. Ferroelectric and magnetic crystals are also characterized by the direction of their electric and magnetic moments, respectively. The corresponding lattices may not necessarily coincide with the crystallographic ones, and they may possibly be mutually incommensurate. The crystal structure of an actual crystal is quite variable, thus opening ways for numerous practical applications. Speciﬁc branches of the physics of solids are dedicated to their description (see Crystal physics). The concept of crystal structure also includes various lattice defects: point defects (such as vacancies, interstitional or substitutional impurity atoms, atomic clusters); linear defects (dislocations); two-dimensional defects (stacking faults, twins, etc.). When studying the crystal structure of solid solutions one has to know the distribution of atoms (ions, molecules) of various types in their sublattices. Crystal structure also includes describing the physical composition and parameters of structural elements (grains, cells, and blocks) and various other factors.

The main techniques for studying crystal structures are X-ray diffraction structural analysis, neutron diffraction, and electron diffraction. CRYSTAL SYMMETRY, microscopic crystal symmetry

Geometrical regularity in the spatial arrangement of particles (atoms, ions, molecules, complexes), composing a crystal. One can characterize the symmetry of a crystal by the totality of all spatial transformations (x , y , z ) = f (x, y, z), which bring the crystal into coincidence with itself. From all conceivable transformations it is sufﬁcient to restrict attention to linear ones, and not necessarily to all of these, but only to deformationfree types, i.e. to linear orthogonal transformations that preserve the lengths of segments and angles between them: (x , y , z ) = α(x, y, z) + (x0 , y0 , z0 ), where α is the transformation matrix. The determinant D = |α| in this case can have only two values D = ±1. The transformations with D = 1 are called proper transformations, and all of them involve rotational spatial displacements (i.e. rotations) around some axis through an angle ϕ, while transformations with D = −1 are called improper; the unit improper transformation being inversion (x , y , z ) = (−x, −y, −z). All improper transformations are combinations of proper transformations with inversion. In general a linear transformation can involve a shift or translation, designated by the term (x0 , y0 , z0 ) through a distance appropriate to the crystal structure lattice spacings. If the term (x0 , y0 , z0 ) = 0 there is no translation, and the transformation is either a proper rotation for D = +1, or an improper rotation for D = −1. The three-dimensional periodicity of a crystal automatically sharply restricts the possible angles ϕ of allowed proper (and improper) rotations to ﬁve values: 0◦ , 60◦ , 90◦ , 120◦ and 180◦ . It is customary to express the allowed angles ϕ by the expression ϕ = 2π/n, and in the international notation to designate proper rotations by the ﬁve integers: n = 1, 2, 3, 4, 6. Improper rotations are ¯ 2¯ = m, 3, ¯ 4, ¯ 6, ¯ where m is the designated by 1, symbol for a mirror reﬂection in a plane. In the older Schönﬂies notation the proper and improper rotations are designated, respectively, by C1 , C2 , C3 , C4 , C6 , I , S2 = σ , S3 , S4 , S6 . There are

CRYSTAL SYSTEM

two special combined rotation-translation symmetry operations: (a) a screw rotation which is a rotation by 2π/n combined with a translation by half a lattice spacing along the rotation axis, and (b) a glide reﬂection which is a reﬂection in a plane combined with a translation by half a lattice spacing parallel to the plane. The complete set of all available symmetry transformations of a crystal form the space group of the crystal (called Fedorov group in the Russian literature). It is discrete, but with an inﬁnite set of elements, because translation through all possible periods is endless. There exist 230 possible space groups, and they are described explicitly in the International Tables for Crystallography. Also important in the physics of crystals are ﬁnite groups containing only proper (and possibly improper) rotational elements (without translations) which are called crystal classes or point groups, and their number is only 32. In three dimensional space there are only 14 translational groups which contain no rotational elements. A set of points invariant under translation form a crystal lattice (Bravais lattice). Each space group has associated with it a point group and a crystal lattice. When describing the symmetry of magnetic (magnetically ordered) crystals (see Magnetism), the situation becomes complicated, since transforming a crystal into itself requires matching not only coordinates of individual identical atoms, but also the directions of their atomic magnetic moments (spins). The Shubnikov extension of symmetry theory to the symmetry of magnetic crystals involves the addition of the non-spatial operation R of spin reversal (see Shubnikov groups). The addition of this new symmetry element permits one to construct 1651 space (Shubnikov)

259

groups, 122 point groups and 36 translational magnetic symmetry groups (see also Antisymmetry). A further generalization brought about the appearance of the theory of colored symmetry, and the creation of many additional colored symmetry groups. All these types of groups ﬁnd use in solid state physics. Concerning macroscopic physical properties (optical, electrical, mechanical, magnetic, etc.), crystals behave as media that are homogeneous, but anisotropic (see Anisotropy of crystals); and the discreteness of their atomic structure is not signiﬁcant. Because of this only the rotational symmetry of a crystal, i.e. its point group, is of importance for the macroscopic directionally dependent properties described by tensors of different ranks. Then the distinction between crystals by their differences in symmetry ﬁnds its expression in the intrinsic symmetry of tensors for different physical properties. The literature provides information on the speciﬁc forms of various tensors of many ranks for all 32 of the crystallographic point groups.

CRYSTAL SYSTEM

The classiﬁcation of crystals in accordance with their crystallographic coordinate system, i.e. by the metric represented by the set of independent linear (a, b, c) and angular (α, β, γ ) crystal lattice constants. It is possible to choose seven different unit cells with the same number of crystal systems corresponding to them (see Table 1). The concept of syngony (in common use in the Russian literature) coincides with the concept of crystal system for all crystal systems except the hexagonal.

Table 1. Unit cell shapes and metric parameters for the seven crystal systems Crystal system

Shape of unit cell

Metric parameters

Triclinic Monoclinic Orthorhombic Tetragonal Hexagonal Trigonal Cubic

Oblique-angled parallelepiped Straight prism with parallelogram in base Right-angle parallelepiped Right-angle parallelepiped with square in base Prism with base in rhombic shape, γ = 120◦ Rhombohedron Cube

a, b, c, α, β, γ a, b, c, β a, b, c a, c a, c a, α a

260

CRYSTAL, THREAD-LIKE

CRYSTAL, THREAD-LIKE See Thread-like crystals. CUBIC SYSTEM A crystallographic system deﬁned by the presence of four third-order symmetry axes (C3 ) in crystals with cubic symmetry. The unit cell of the

system is a cube with lattice parameter a. The coordinate axes of a cubic system contain 4, 4, and 2 (i.e. C4 , S4 , and C2 ) symmetry elements. This system includes three Bravais lattices (primitive, body-centered, face-centered), ﬁve point groups (T , Th , Td , O, Oh ), and 36 space groups (see Crystal symmetry). CUMULATIVE EFFECT

Accumulation is a process of building up the energy ﬂux density in a medium by focusing the ﬂows of energy. It is achieved either through speciﬁc shaping of an elongated energy source, or through the interaction of shock waves. This effect is usually produced using explosives. In solids this may be realized in several ways, as follows. Cumulative jets are formed by compressing metal linings placed into the cumulative cavities in explosive charges. The shape of the lining may be hemispherical, conical, parabolic, hyperbolic, etc. Compression concentrates the principal part of the explosive energy into a thin internal layer of the lining so that this layer forms a cumulative jet. The mass of metal transformed into the jet may reach 6–20% of the total mass of the lining, and the energy density in the jet may reach 106 MJ/m3 . Shock wave collision. During a frontal collision of shock waves in a solid (see Explosion) each element of the solid is sequentially compressed ﬁrst by the incident and then by the reﬂected shock wave. As a result, pressures in the area of the reﬂected shock wave exceed those in the incident wave by a factor of several times, while temperatures remain comparatively low, that is lower than those resulting from compression by a single shock wave. During a glancing collision of shock waves that meet at a certain angle a triple shock wave conﬁguration forms, and pressures in its forward wave signiﬁcantly exceed those produced during a frontal collision. By means of this technique a pressure of 1.8 TPa was achieved in copper samples.

Cumulation in a medium with varying density. When a shock wave exceeding a critical value passes through a system of gradually tapering alternating layers of light and heavy material its propagation develops into a periodic selfreinforcing process (see Self-similarity) that results in the unlimited growth of pressure at its front. CUNICO

Hard magnetic material based on the Cu–Ni– Co system. A high-coercive state is achieved upon quenching from 1100 ◦ C and tempering at 625 ◦ C. Cunico alloys are readily plastically deformable, so they are employed for the manufacture of permanent magnets of a complicated shape. For properties, see Table 1 in Hard magnetic materials. CUNIFE

Hard magnetic material based on the Cu–Ni– Fe system. A high-coercive state is achieved upon quenching from 1100 ◦ C, tempering at 700 ◦ C, applying cold strain with high compression, and tempering at 650 ◦ C. The strain induces uniaxial magnetic anisotropy along the rolling or drawing direction. Cunife alloys are used as thin wires or stampings. For properties, see Table 1 in Hard magnetic materials. CURIE GROUP

See Limiting symmetry groups. CURIE LAW (1895)

Temperature dependence of the magnetic susceptibility, χ = C/T , in many paramagnets, where C is the Curie constant (C > 0). All gases in which the atoms, molecules, or ions have permanent magnetic moments follow the Curie law, as well as dilute liquid solutions of transition metal ions, as well as crystals of compounds of these elements with non-metallic bonding. It holds for temperatures at which the thermal energy signiﬁcantly exceeds the energy of interaction of neighboring ionic magnetic moments with each other, and with the external magnetic ﬁeld.

CURIUM

For subsystem properties, the case

CURIE POINT, Curie temperature

The point (temperature TC ) of a second-order phase transition. Examples of a Curie point are the temperatures TC of magnetic phase transitions, ferroelectric phase transitions, structural phase transitions, and other phase transitions in solids. Special names are used for certain transitions, such as the Néel point for the antiferromagnetic Curie point. CURIE PRINCIPLE (P. Curie, 1984)

This principle deals with the symmetric aspect of the causality principle. Namely, the symmetry of a system of causes is (abstractly) preserved in the symmetry of the outcomes. This principle is a philosophical generalization of the Neumann– Minnegerode–Curie principle which states that the symmetry of physical properties of a system made of a material object (e.g., a crystal) and of an external action is not lower than the intersection (a general subgroup) of the groups of symmetry of the object and action. The Curie principle holds for all deterministic systems, to which the notion of symmetry can be applied. A modern formulation of the Curie principle establishes a homomorphism relation in the particular case of an isomorphism between the symmetry groups of a system of causes Gcsys and a system of outcomes Gout sys : Gout sys =

!

sym

Gout j Gout

↔

!

sym

Gcj Gc

= Gcsys .

For a homogeneous system, parts of which are connected by some symmetrizer Gsym , its symmetry is deﬁned by the intersection of the sym" metry groups of its parts, Gj = G1 ∩ G2 ∩ · · ·, multiplied by Gsym (the Shubnikov theorem). For an inhomogeneous system, Gsym reduces to identity and the " system symmetry is deﬁned by the intersection Gj (the Curie theorem). Taking, e.g., the interaction of an object with an external action as the cause of a physical phenomenon, we ph can ﬁnd the symmetry group Gj of a systemsym

atic phenomenon (for Gc case,

= 1), or in a particular

Gobject ∩ Gaction = Gcsys .

261

ph

c Gout j ↔ Gj ← Gsys sym

is possible if Gc = 1 (the Wigner theorem). This systematic formulation explains violations of the Curie principle associated with the incompleteness of a given system of causes, an inexact deﬁnition of symmetry of the system components, or with using the Curie theorem instead of the Shubnikov theorem. CURIE–WEISS LAW (P. Curie, P. Weiss, 1907) The temperature dependence of the susceptibility χ of ordered systems above the point of their transition to an ordered phase at the Curie point TC

has the form: χ = χ0 +

C , T −θ

where C is the Curie constant, χ0 is the temperature independent part of the susceptibility, and θ is the characteristic temperature. For the magnetic susceptibility χ of paramagnets, or ferromagnets in their paramagnetic phase above TC , as well as for the dielectric susceptibility of ferroelectrics and other materials, θ is called the Weiss temperature, or sometimes the Curie–Weiss temperature. The value of θ depends on particle interactions, and may differ appreciably from TC (see also Dielectric constant). In the case of antiferromagnets (or antiferroelectrics) and virtual ferroelectrics the value of θ may become negative. The Curie–Weiss law holds for the range of temperatures in which the ﬂuctuations are not critical uctuations, that is for (T − TC )/TC Gi, where Gi is the Ginzburg number. CURIUM, Cm

A chemical element of Group III of the periodic system with atomic number 96 and atomic mass 247.07; it is a member of the actinide family. 15 isotopes are known with mass numbers 238 to 252, none of them being stable. The electronic conﬁguration of the outer shells is 5f 7 6d 1 7s 2 . The ionization energy is 6.09 eV. Atomic radius is 0.1749 nm; radii of Cm3+ and Cm4+ ions are 0.0946 and 0.0886 nm, respectively. Oxidation state is +3 (more rarely, +4, +6).

262

CURRENT CARRIER DRIFT

In the free form, curium is a soft silvery-white metal. It exists in two allotropic modiﬁcations:

a low-temperature α-Cm below 873 K, and a high-temperature form β-Cm. The α-Cm variety has a double hexagonal close-packed crystal lattice with alternation of layers according to the 4 ), ABAC. . . scheme; space group P 63 /mmc (D6h a = 0.344 nm, c ≈ 1.16 nm. The β-Cm form has a face-centered cubic lattice, space group F m3m (Oh5 ), a = 0.5039 nm upon hardening. Density of α-Cm is 13.51 g/cm3 ; T melting = 1620 K, T boiling is about 3380 K; speciﬁc heat cp = 27.6 J·mole−1 ·K−1 ; heat of melting is 14.64 kJ/mole, heat of sublimation is 372.6 kJ/mole. Below the Néel point T N = 52 K, α-Cm transforms from the paramagnetic state to the antiferromagnetic one (see Antiferromagnetism); below the critical temperature T c = 205 K, β-Cm is a ferrimagnet, or has a noncollinear magnetic structure. Targets from isotopes 246 Cm and 248 Cm are used in the synthesis of the heavier transuranium elements by bombardment with the multicharged ions. High heat release in the preparations from the isotopes 244 Cm and 242 Cm caused by their α-decay suggests the possibility of using these nuclides to produce small-size nuclear electric current sources that persist for several years (e.g., in onboard space systems). CURRENT CARRIER DRIFT, charge carrier drift

A directed movement of charge carriers in semiconductors under the action of external ﬁelds

imposed on their disordered (thermal) motion. The current density resulting from the charge carrier drift in the electric ﬁeld E (drift current) is j = σ E, where the electrical conductivity σ = e(μe n + μh p), n and p are the concentrations of the conduction electrons and holes, respectively, and μe and μh are their mobilities (see Mobility of current carriers). The total conduction current density is the sum of the drift current, the diffusion current, and the thermoelectric current arising from the presence of a temperature gradient. The charge carrier drift can also result from the carrying along of carriers by either an ultrasonic wave (see Acousto-electric effect) or an electromagnetic wave (radio electric effect, light electric effect). In this event the drift involves nonequilibrium carriers, and therefore it becomes complicated by the

appearance of bulk charges whose ﬁeld should be taken into account in addition to the external ﬁeld and the recombination of current carriers. The motion of injected nonequilibrium carriers (see Injection of current carriers) in the external electric ﬁeld is described by so-called ambipolar mobility μa =

μe μh |n − p| , μe n + μh p

which, in general, differs from μe and μh . For an intrinsic semiconductor n = p and μa = 0; for an n-type semiconductor n p, μa = μh ; and for a p-type semiconductor p n, μa = μe , which means that in an impurity semiconductor μa coincides closely with the mobility of the minority carriers. The velocity of the grouping of nonequilibrium carriers in an external ﬁeld E is equal to μa E. An important characteristic of charge carrier drift is its drift length l, which is the distance that the carriers traverse in going from their point of generation (see Generation of current carriers) to their recombination point. This length has the value l = μEτ , where τ is the lifetime of the nonequilibrium carriers. The method for measuring the drift length is the same as that for measuring the diffusion length. In anisotropic crystals the direction of the drift can differ from that of the electric ﬁeld (since mobilities are tensors). In strong electric ﬁelds the drift can be anisotropic even in isotropic (cubic) many-valley semiconductors. In the presence of a transverse magnetic ﬁeld the drift direction does not coincide with the electric ﬁeld direction. In a strong magnetic ﬁeld B normal to the external electric ﬁeld E satisfying the condition cB E, the charge carriers drift in the direction normal to both E and B with the velocity v = E/B that does not depend on the carrier mobility. A circular motion of the carriers at the cyclotron frequency is superimposed on this drift. CURRENT CARRIER GENERATION See Generation of current carriers. CURRENT CARRIER MOBILITY See Mobility of current carriers. CURRENT CARRIER RECOMBINATION See Recombination.

CURRENT CARRIER SCATTERING

CURRENT CARRIERS, charge carriers Mobile charged particles and quasi-particles.

In an external electric ﬁeld, the random motion of the current carriers acquires a directional component (see Current carrier drift), so that an electric current ﬂows. The current carriers in metals are usually electrons of the conduction band, but when this band is more than half full, the current carrying role is better described in terms of holes in this band. In metals the concentration of current carriers is about 1022 –1023 cm−3 , i.e. is of the order of the number of atoms in the crystal itself, while the mobility μ of conduction electrons usually lies within 105 –107 cm2 ·V−1 ·s−1 ). However, in super-pure metals, it may increase by 3–4 orders of magnitude (see Mobility of current carriers). The carriers of current in semiconductors are usually electrons in the conduction band and holes in the valence band. Their concentrations, n (electrons) and p (holes), may vary by many orders of magnitude from sample to sample of the same material, depending on the concentration of impurity atoms (donors, acceptors), intrinsic defects, the temperature, and external actions. Dark current carriers are those which exist in semiconductors in the absence of photoexcitation; equilibrium current carriers are those present when thermodynamic equilibrium exists between allowed energy bands and local electronic levels. For the case n > p at equilibrium, the majority current carriers are electrons, otherwise they are holes. Nonequilibrium current carriers appear when the electron subsystem is variously excited. The nonequilibrium concentration of minority current carriers may be easily raised far above its equilibrium value. It is controlled by the efﬁciency of the injection of minority current carriers into the band, and by their lifetime in that band. In semiconductors, the mobility of carriers usually lies within the range 102 –104 cm2 ·V−1 ·s−1 . The electron (hole) component of conductivity may include impurity conductivity only, without any input from the allowed band (see Impurity band, Hopping conductivity), and the carrier mobility μ may then remain much lower than 1 cm2 ·V−1 ·s−1 . The interaction of free electrons or holes with the surrounding atoms of the crystal may result in the formation of polarons and ﬂuctuation states of the current carriers (see Polaron, Fluctuon). In insulators the role of charge carriers may be played

263

by interstitial ions of either intrinsic or impurity atoms, or by charged vacancies (see Ionic conductivity). CURRENT CARRIER SCATTERING in crystals A transition of an electron (or hole) between

states described by Bloch wave functions under the action of a perturbation of the periodic crystal e ld. There are two types of such perturbations that inﬂuence the mechanism of the scattering. The ﬁrst type includes static defects of the crystal lattice: impurity atoms, vacancies, dislocations, crystallite boundaries, and the external surface of the specimen (see Surface scattering). The second type includes dynamic perturbations: phonons, other electrons, magnons, etc. The interaction of current carriers with the perturbation of the periodicity is described by a Hamiltonian H = H − H0 , where H is the Hamiltonian of the actual crystal and H0 is the Hamiltonian of an ideal crystal. This results in electronic transitions between the states with quasi-wave vectors k and k and energies ε(k) and ε(k ). Provided |ε(k ) − ε(k)| ε(k) then we have quasi-elastic (elastic) scattering. To each current-carrier scattering mechanism there corresponds a separate Hamiltonian H , a probability W (k, k ) of the transition from state k to state k , and a relaxation time for quasi-momentum τp , provided such a variable may be introduced. Calculations of W (k, k ) are usually carried out within ﬁrst-order perturbation theory (|H | H , the Born approximation), and Δt τp , where Δt is the action time for the perturbation in the elementary scattering event. Scattering hampers directional motions of electrons either in the external electric ﬁeld or under the effect of a temperature gradient, these motions generating the electric current and the energy ﬂux, respectively. The quantity W (k, k ) enters the collision integral in the Boltzmann kinetic equation (see Boltzmann equation), its solution permitting the determination of kinetic coefﬁcients. Among the latter are, in particular, the mobility of current carriers μ and the Hall constant (see Galvanomagnetic effects). The solution of that equation simpliﬁes if the variable τp may be introduced. For the simultaneous action of several scattering −1 mechanisms the values Wi (k, k ) and τpi are

summed: 1/tp = i (1/τpi ). In some cases this

264

CURRENT CARRIER SCATTERING

summation process extends to 1/μ = i (1/μi ) and ρ = i ρi (Matthiessen rule for resistivities ρI ), which hold for τpi independent of k. Provided W (k, k ) depends on the angle between k and k only, the microparticle scattering is called isotropic scattering, and when it also depends on the directions of k and k it is anisotropic scattering. The relaxation time is a tensor in the latter case. Current carrier scattering in semiconductors. Besides the mechanism of scattering proper, this effect is controlled by the dispersion law for the current carriers. When k and k belong to the same valley the process is called intravalley scattering, otherwise it is designated intervalley scattering. If one may express τp ∝ es and μ ∝ T α then the quantities s and α control the scattering process. During the scattering of electrons by lattice vibrations (phonons) a phonon with an energy ω(q) and a quasi-wave number q (ω is the frequency) is either emitted or absorbed in an elementary scattering event. The conservation laws of energy ε(k) = ε(k ) ± ω(q) and quasi-momentum k = k ± q + b are then obeyed. The “minus” sign here corresponds to the absorption of a phonon, while “plus” corresponds to its emission, and b is a reciprocal lattice vector. Processes with b = 0 are the so-called ﬂip-over or Umklapp processes. It is important to account for them when (k − k ) lies outside the ﬁrst Brillouin zone, where b brings q back into the ﬁrst zone. Umklapp processes are insigniﬁcant for valleys in the center of the ﬁrst Brillouin zone (see Many-valley semiconductors). Acoustic vibrations of atoms deform the crystal, changing the energy of the bottom of the conduction band, and produce a scattering acoustic strain potential = ε Δv/v , where ε is the strain potenHac 1 0 1 tial constant (sometimes the strain potential itself), and Δv/v0 is the relative change of a given semiconductor volume, e.g., a unit cell. holds for an The above expression for Hac isotropic electron dispersion law only, and for an extremum at the center of curvature of the ﬁrst Brillouin zone. In the general case the strain potential constant is a tensor (strain potential tensor) to the strain. When T > T = that relates Hac 0 2 mn u /kB ≈ 1 K, where mn is the effective mass of the electron, u is the sound velocity, kB is the

Boltzmann constant, the scattering is quasi-elastic, so that only the phonons with q < 2k take part in it. The Planck distribution function for them may be approximated by the classical expression kB T / that corresponds to an equilibrium energy distribution over the degrees of freedom, so that these are equidistributed phonons. In the simplest case of an isotropic parabolic dispersion law for ε(k) we have s = −1/2, α = −3/2, r = 3π/8 = 1.18. Optical vibrations of atoms produce a scattering optical strain potential (scattering by nonpolar optical phonons). When kB T ω0 , where ω0 is the frequency of an optical phonon, the scattering is elastic, s = −1/2, α = −3/2, r = 3π/8 = 1.18. At all other temperatures the scattering becomes inelastic. Provided, however, that the dispersion law is isotropic (or close to isotropic and averaged over directions), the equality W (k, k ) = W (k, −k ) makes it possible to introduce τp . If kB T ω0 , μ ∝ τp ∝ exp[ω0 /(kB T )], r = 1. Only these two cases of scattering by phonons are possible in nonpolar crystals such as Ge and Si. In polar crystals (e.g., AIII BV ) scattering by the polar optical potential resulting from the lattice polarization (see Polarization of insulator) contributes to the optical vibrations of the atoms (scattering by polar optical phonons). Such scattering may be stronger than scattering from acoustic and optical deformation potentials. It is elastic for kB T ω0 and s = 1/2, α = −1/2, r = 45π/128 = 1.105, and becomes inelastic at other temperatures. However, when kB T ω0 one may introduce τp since electrons can only absorb an optical phonons in a weak electric ﬁeld. Moreover, having absorbed the optical phonon, the electron emits it almost instantaneously (the probability ratio then becomes exp[ω0 /(kB T )] 1. The electron energy undergoes almost no change during such a composite scattering event, while k does change. We have μ ∝ τp ∝ exp[ω0 /(kB T )], r = 1 in the absence of degeneracy. In crystals with partial ionic bonding acoustic vibrations may also produce, beside the deformation potential, a piezoelectric scattering potential, provided the crystal possesses no center of symmetry (e.g., in AIII BV , AII BVI semiconductors, see Piezoelectricity). A piezoelectric constant enters the formulae describing scattering by that

CURRENT CARRIER SCATTERING

potential, and s = 1/2, α = −1/2, r = 45π/128 = 1.105 for the case. At low temperatures the phonon gas is rareﬁed and the main effect may consist in scattering by impurity atoms; the scattering in that case is elastic because of the great difference between the masses of the electron and the atom. Scattering from ionized impurities is similar to the Rutherford scattering of α-particles. The Conwell–Weisskopf formula (E.M. Conwell, V.F. Weisskopf, 1950) obtained for μ for that kind of scattering does not take into account the screening by free electrons of the ﬁeld produced by the impurity ions (see Electric charge screening), while the Brooks– Herring formula does. In both cases, and to within the accuracy of certain factors slowly changing with temperature T and the impurity concentration N , we have τp ∝ e3/2 /N , μ ∝ T 3/2 /N , r = 315π/512 = 1.93. Scattering by neutral impurities is similar to electron scattering by atoms of hydrogen: s = 0, α = 0, r = 1. The corresponding formula for τp is called the Erginsoy formula (C. Erginsoy, 1950). In the case of scattering from point defects with a short-range δ-function potential α = −1.2, s = −1.2. In all the above theories the scattering of current carriers is assumed to be incoherent scattering, with the assumption of no interference between electron waves scattered by different impurity atoms. This is generally true for a random distribution of impurity atoms. The above dependences of the mobility μ on the temperature T are usually not observed experimentally, since they were obtained from idealized models. The reason for such a pronounced disagreement between theory and experiment may lie in a dependence of mn and of the deformation potential on the temperature T . Also, the band may deviate from a parabolic shape, the electrons may exhibit partial degeneracy, etc. For example, in the case of scattering by phonons in germanium, α = −1.66 for electrons and α = −2.33 for holes. Electron–electron scattering does not change the total quasi-momentum of the electron gas, and hence has not affect on either the current or μ. However, provided some other scattering mechanism is simultaneously at work, characterized, as it were, by a τp (ε), both the current and μ will change because of energy redistribution among the electrons. This effect is characterized by the

265

electron–electron scattering time, τee . When the electrons collide with each other, a noticeable exchange of both quasi-momentum and energy takes place, because of the equality of their masses, and τee controls the rate of both processes. In the absence of degeneracy we have τee ∝ n−1 , where n is the electron concentration. The electron–hole scattering is signiﬁcant for high concentrations of current carriers (high temperatures, high levels of injection of electrons). It is similar to scattering by ionized impurities when the ionic charge is opposite to that of the scattered carriers. Scattering by dislocations occurs due to the interaction of current carriers with charged dislocation ﬁlaments, and the deformation potential produced by the ﬁeld of strained dislocations. When the scattering center has a magnetic moment then electron spin- ip scattering becomes possible, which leads to the Kondo effect. The energy relaxation time, τe , may often be represented in the form te ∝ el , where the value of l depends on the scattering mechanism. We have l = −1/2 for the acoustic deformation potential, l = 1/2 for the optical, l = 3/2 for the polar optical, and l = 1/2 for the acoustic piezoelectric potential. The inequality τp τe holds for the averages of τp and τe in the case of quasi-elastic scattering. Scattering of current carriers in metals. This manifests itself in the principal kinetic properties of the metal, its electrical conductivity and thermal conductivity. The electrical resistance is related to the relaxation of the electron quasi-momentum, while the thermal resistance arises from both momentum and energy relaxation. When the momentum relaxation prevails, the Wiedemann–Franz law 2 /(3e2 ), where κ is the elecholds: κ/(σ T ) = π 2 kB tronic thermal conductivity and σ is the electrical conductivity. The scattering of current carriers in metals is also inﬂuenced by the shape of the Fermi surface. In the case of electron–phonon scattering, determining the explicit form of the Hamiltonian H is a difﬁcult problem, since the displacement of ions leads to a signiﬁcant restructuring of the electronic wave functions. At the same time semiempirical techniques are available that make it possible to relate matrix elements of the Hamiltonian to the structure of the Fermi surface. The most well-known one is based on combining the model of rigid (undeformable) ions

266

CURRENT CARRIER SCATTERING

with the pseudopotential method. It is not difﬁcult to demonstrate, without falling back to model considerations, that the squared matrix element of the Hamiltonian H is proportional to the phonon momentum to ﬁrst order for the case of scattering from long-wave vibrations. The mechanism of electron–phonon relaxation depends qualitatively on the relation between the momentum of thermal phonons q and the typical size PF of the Fermi surface (note that an intermediate range PF1 < q < PF2 is also realized in Bi, PF1 and PF2 being the major and the minor semiaxes of the ellipsoidal Fermi surface). Let us introduce the maximum energy of the phonons that can interact with electrons: θ = uPF . The ratio θ/kB in typical metals is of the order of the Debye temperature. At high temperatures we have kB T θ and the phonons with energy of the order of θ and momentum q ≈ PF are important. The number of such phonons and, accordingly, the probability of electron–phonon collisions, are proportional to the temperature T . The electrical resistance is, correspondingly, ρ ∝ T . Since the characteristic energy scale of the change in the Fermi distribution function for electrons (see Fermi–Dirac statistics) kB T is much larger than the phonon energy, such collisions are quasi-elastic, and the Wiedemann–Franz law holds. At low temperatures kB T θ and phonons with energy of the order of kB T and momentum q = kB T /u = PF kB T /θ start to play the decisive role. In this particular case energy relaxation occurs during a single collision event. A signiﬁcant change in the electron momentum ω requires [PF /(q)]2 = [θ/(kB T )]2 collisions. Such a relaxation is essentially a diffusion of electrons over the Fermi surface that proceeds with a typical step of q PF . Due to the laws of conservation of energy and momentum such an electron may only interact with those phonons that have their momenta normal to the electron velocity vector, the number of such phonons being proportional to T 2 . In addition, the squared matrix element of the electron–phonon interaction is proportional to the ﬁrst power, q ∝ T . As a result, the energy relaxation time at low temperatures is te ∝ T −3 , while the transport (pulse) time is proportional to τp ≈ τe [θ/(kB T )]2 ≈ T −5 . The corresponding electrical resistivity follows the Bloch law, ρ ∝ T 5 . Naturally, the Wiedemann–Franz law now no longer

holds. Strictly speaking, the above refers to compensated metals (with equal numbers of electrons and holes), or to metals with open Fermi surfaces. For an uncompensated metal the relaxation of total momentum at low temperatures is controlled by electron–phonon collisions, accompanied by Umklapp processes. Moreover, such processes are only possible in the regions where closed Fermi surfaces come closest to each other, the so-called hot spots or hollows. The transport relaxation time, roughly speaking, is equal to the sum of the time span of transitions across the Fermi surface to one of the hollows by diffusion, plus the time an electron takes to ﬂip over or undergo an Umklapp process in a hollow. Usually the ﬁrst time span signiﬁcantly exceeds the second (Umklapp processes proceed relatively readily), so that the Bloch law remains valid. Umklapp processes may control momentum relaxation only in the range of extremely low temperatures (about 1 K), resulting in an exponential temperature dependence of the electrical resistivity against the background of the predominant inﬂuence of electron–impurity scattering. Electron–electron collisions. Only electrons from regions where the Fermi distribution is blurred or diffuse may take part in such collisions, due to the Pauli principle and the conservation of energy law. In other words, a given electron may only collide with a small fraction of the conduction electrons, of the order of kB T /εF (εF is the Fermi energy), since the number of available states is proportional to kB T /εF . (After one of the electrons enters the diffuse range, another appears automatically, due to energy conservation during their collisions.) Thus, taking into account the Pauli principle lowers the probability of an electron–electron collision by a factor of [εF /(kB T )]−2 (see Fermi liquid). One should also take account of the fact that the screening radius in a typical metal is of the order of the lattice constant, and as a result, the mean free path for electron–electron collisions is lee ≈ a[εF /(kB T )]2 . Umklapp processes during electron–electron collisions are possible when the Fermi surface crosses a plane normal to a certain vector b of the reciprocal lattice located a distance b/4 from the center of the Brillouin zone. The law ρ ∝ T 2 might manifest itself at low enough temperatures when one could neglect the input from

CURRENT STATES IN METALS

electron–phonon scattering, but there is no reliable experimental evidence for this. Meanwhile, electron–electron collisions play a role during the absorption of electromagnetic waves in metals in the near-IR spectral range. Having absorbed an electromagnetic quantum with energy ω kB T the electron may interact with other electrons in a layer of thickness ω. Calculations result in a substitution in the expression for the probability 2 T 2 factor is of electron–electron collisions: the kB 2 2 2 replaced by kB T + [ω/(2π)] . This does not apply at T = 0 where everything is in the ground state. Scattering from static defects is usually elastic, hence the collision probability does not depend on the temperature, and the Wiedemann–Franz law holds. Local defects such as impurity atoms significantly perturb the crystal ﬁeld at distances of the order of a lattice constant a. The ﬁeld of a charged impurity is screened by electrons, the screening radius (Debye radius) in a typical metal also being of the order of a. Therefore, the scattering crosssection is of the order of a 2 , and depends on the relatively weak inﬂuence of the local defects. The mean free path is led ∝ aC −1 , where C is the number of local defects divided by the number of cells in the crystal lattice. CURRENT, CRITICAL See Critical currents. CURRENT, ELECTRIC See Electric current. CURRENT FILAMENTATION, current channeling

Electric current ﬂow in a sample with a nonuniform distribution over the cross-section, i.e. high densities along some channels (ﬁlaments), and low or zero densities along neighboring parallel paths. The phenomenon of current ﬁlamentation may result from an S-shaped current–voltage characteristic. Such a characteristic can arise from certain mechanisms of current carrier scattering in solids. In addition an S-shaped characteristic in a uniform semiconductor may arise from the release of Joule heat (overheating instability); when a temperature increase caused by the current ﬂow leads to additional electron transitions from local electron levels in the conduction band then the current

267

can increase still further, with a further rise in the lattice temperature. The channeling often brings about irreversible processes in the current channel, which could put the device out of operation. If the channeling associated with an S-shaped characteristic happens at high frequencies it may be used for the generation of super-high frequency oscillations (harmonics), as occurs in various types of diodes (e.g., trapped plasma avalanche triggered transit diode, tunnel diode, impact ionization avalanche transit time diode). Besides, the pinch effect may be responsible for current channeling in semiconductors (see Magnetic pressure). Also this channeling may be observed in pure metals at low temperatures through the magnetodynamic mechanism of nonlinearity (see Magnetodynamic nonlinearity). CURRENT, PERSISTENT See Persistent current. CURRENT STATES IN METALS

A hysteresis effect (in an external magnetic ﬁeld B0 ) of electric current rectiﬁcation, and the excitation of a static magnetic moment in the sample when irradiating the latter by an rf (radio wave) of a high amplitude Brf . This takes place at the quasi-static limit ωτ 1 (here ω is the rf frequency; τ is the electron characteristic lifetime) of the anomalous skin-effect, with B0 parallel to the rf magnetic ﬁeld vector Brf . The current states are excited when Brf exceeds a threshold value Bcr ∼ 0.1–1 mT that is determined by ω, the mean free path l, and the character of the electron surface scattering. For diffusion scattering Bcr ∝ ω−1/3 l −2 . In the ideal case of specular reﬂection the current states do not emerge. At the regime of strong nonlinearity Brf > Bcr , the magnetic moment does not vanish even at B0 = 0. For growing Brf , the hysteresis loop approaches a universal curve which is determined only by amplitude Brf , and does not depend on the electrodynamic properties of the metal. The excitation of current states is stimulated by sharp conductivity jumps during the rf period which are due to the appearance and disappearance of trapped electrons in the skin-layer (see Magnetodynamic nonlinearity).

268

CURRENT STATES IN SUPERCONDUCTORS

CURRENT STATES IN SUPERCONDUCTORS

States with a ﬁnite current I at zero voltage which correspond to an inﬁnite electrical conductivity. The current states are metastable under the condition I > Ic where Ic is the temperaturedependent critical current which goes to zero at the transition point Tc . In this case, in the vicinity of Tc , we have Ic = const(Tc − T )3/2 (Bardeen law). The energy E is related with the current as E = Lk I 2 /2, where Lk is the kinetic inductance of the superconductor. Strictly speaking, a current state as a metastable state has a ﬁnite lifetime, but for macroscopic superconducting rings the persistent current decay times are so long that it is reasonable to speak about an “inﬁnite conductivity”. The existence of current states is the consequence of the macroscopic quantum coherence of electronic states of the superconductor which are described by a uniﬁed wave function ψ = F eiϕ . In this case the current state is given by the magnitude of phase gradient ∇ϕ according to j = ns evs , vs =

1 (∇ϕ − 2eA), 2m

where vs is the super uid velocity (velocity of motion of condensate); ns is the temperaturedependent concentration of superconducting electrons (ns /2 is the concentration of Cooper pairs). For a pure superconductor ns = n at T = 0, where n is the total concentration of electrons; for a superconducting alloy with a mean free path l less than the coherence length ξ0 , ns = nl/ξ0 at T = 0. As vs grows, the value ns decreases so that the dependence j (vs ) takes the shape of a curve with a maximum (“depairing curve”). The critical depairing current jc is determined as the maximum of the dependence j (vs ), and is estimated as jc ∼ ns (vs = 0)evc (here vc = Δ/pF is the critical velocity). This estimate gives a critical current density value of jc ∼ 109 A/cm2 which is achieved in thin superconducting ﬁlms or ﬁlaments (with thickness or diameter less than ξ0 ). In bulk samples the depairing current is not reached, as a rule, and the critical current is determined by the decay of the superconductive state via the intrinsic magnetic ﬁeld of the current in type I superconductors (Silsbee rule, F.B. Silsbee, 1916),

N-shaped (left) and S-shaped (right) current versus voltage characteristics.

or by the Abrikosov mechanism of vortex pinning in type II superconductors. The current states also occur at superconducting tunnel junctions (dc Josephson effect). In this case the factor which determines the current through this transition is the phase difference ϕ1 − ϕ2 of the condensate wave functions of the two superconductors: I = Ic sin(ϕ1 − ϕ2 ). CURRENT–VOLTAGE CHARACTERISTIC

The dependence of the electrical current I on the voltage V applied to an electric circuit element. If the element resistance does not depend on the current then the current–voltage characteristic (CVC) is a straight line (Ohm’s law). The I versus V characteristics of some circuit elements can have sections which are nonlinear with various shapes. In semiconductors the appearance of non-linear sections can result from the limitations of current through the contact arising from the dependence of the emission ability of the contact on the presence of regions of space charge, and from the dependence of the current carrier mobility on the electric ﬁeld strength. In some cases a current–voltage characteristic has sections of negative slopes, corresponding to negative resistance dV /dI (see Fig.). Negative resistance means that the conduction occurs under unstable conditions. Fig. left: an I versus V characteristic with an N-shape which is seen in tunnel diodes and in semiconductors containing traps with a speciﬁc dependence of the carrier trapping on their energy. Right: an S-shape characteristic which can result from an “overheating” mechanism, associated with the electron heating, and also from an avalanche breakdown due to impact ionization of impurity atoms.

CYBOTAXIS

CURVATURE TENSOR

Riemann tensor, a 4th rank tensor that characterizes the deviation of the geometry of space from the Euclidean type. The mixed curvature i , is deﬁned through the Christoffel tensor, Rklm i as follows: R i i i symbols Γkl klm = ∂l Γkm − ∂m Γkl + i n n i i Γnl Γkm − Γnm Γkl (here ∂i = ∂/∂x , repeated indices imply summation). The covariant curvature n (where g is the metric tensor Riklm = gin Rklm in tensor) satisﬁes the relations Riklm = −Rkilm = −Rikml = Rlmik ; Riklm + Rilmk + Rimkl = 0. A property of this tensor is that there exists a coordinate system such that the tensor is identically zero when the space is locally Euclidean (i.e. gik may be reduced to the metric tensor of ﬂat space with the corresponding signature via a coordinate transformation in a ﬁnite neighborhood of an arbitrary point). The inverse statement is also valid. Thus, the vanishing of the curvature i provides an invariant criterion for tensor Rklm the Euclidean nature of space that is independent of the choice of coordinate system. This property of the curvature tensor is used in elasticity theory to derive the conditions for the strain compatibility that are equivalent to the vanishing of the curvature tensor formed from the Christoffel symbols which are calculated from the displacement ﬁeld. When the solid contains dislocation and disclination types of defects, which give rise to incompatible deformations, the condition of i = 0 is violated. The solid is compatibility Rklm then internally stressed, i.e. there are tensions in it even in the absence of external loads (see Internal stresses). Such a solid is described by a non-Riemann geometry, with a curvature tensor that differs from zero, and another tensor called n is formed from the Einstein tensor Rkm = Rknm it. Note that Rkm = Bkm , where the so-called “material tensor” Bkm describes the distribution of additional matter that produces incompatible deformations within the body. For example, this relation describes internal stresses in a solid that result from a prescribed density of dislocations (see Dislocation density tensor). CYANIDING

Diffusion saturation of the surface of steel and cast-iron products by nitrogen and carbon simultaneously, generally in melts containing cyanide

269

salts. The thickness of the cyanided layer is 0.05 to 2 mm. Cyaniding increases the surface hardness of the products, their wear resistance, and their endurance limit. Tool steels are cyanided at 450 to 600 ◦ C, structural steels below 950 ◦ C. Cyaniding is distinguished by cementation and nitriding (see Chemical heat treatment) depending on the higher velocity of the process. After the high-temperature cyaniding the products are subjected to hardening and to low-temperature annealing. CYBOTAXIC CLUSTERS Domains with a ﬂuctuation origin having a smectic structure found in a nematic liquid crystal, existing in the vicinity of a nematic–smectic phase transition. Cybotaxic clusters present in the

nematic phase inﬂuence the longitudinal bending and twisting strains. Smectic layers in the cluster should be equidistant. As a result, the Frank elasticity constants K2 and K1 in the neighborhood of the transition in the smectic liquid crystal phase increase directly as the cluster size (see Elasticity of liquid crystals). CYBOTAXIS

Name of a hypothetical three-dimensional arrangement of particles (atoms, molecules) in ﬂuids which are in a state intermediate between one that is completely disordered and one that is crystalline. The term “cybotaxis” was introduced by D. Stewart and R. Morrow (1927). The atoms and molecules in cybotaxes have mobility, but their motion and relative arrangement are not disordered as in the gaseous state. A cybotaxis has no sharply delineated boundary. The lifetime of cybotaxes depends on the composition of the ﬂuid, and the temperature. The basis for introducing the cybotaxis concept was X-ray structure analysis data that reveal that at temperatures slightly above the melting point the arrangement of atoms and molecules in liquids is similar to the arrangement in crystalline solids. It is possible to connect the formation of locally regular clusters in glasses which inherit the structural elements of smelts on quenching, with the presence of cybotaxes in smelts. Cybotaxes are often associated with localized arrangements of molecules in liquid crystals. See also Polycluster amorphous solids, Lebedev crystallite hypothesis, Liquid state models.

270

CYCLIC HEAT TREATMENT

CYCLIC HEAT TREATMENT A heat treatment of metals and alloys involv-

ing periodic heating and cooling of the material. This is employed to induce structural changes that lead to the improvement of mechanical properties. One heating and one cooling event constitute a unit cycle of a cyclic heat treatment. The cycle conﬁguration (i.e. temperature versus time dependence), its parameters (maximum and minimum temperatures of the cycle, heating and cooling rates, exposure time at the maximum temperature of the cycle) and the number of cycles can vary, depending on the type of material being treated, its original condition, and the needed structural changes. A cyclic heat treatment can be carried out so that no phase transitions take place in the temperature range of the cycle. In this case structural changes in the cyclic process account for the plastic deformation due to the thermal stresses which arise as a result of temperature gradients induced by heating and cooling the material. Substantial changes take place in the intragrain dislocation structure, grain interfaces (see Grain boundaries), regions of grains adjacent to interfaces, and the quantity and morphology of particles of phases which gain strength. In particular, the durability of metals and alloys under the conditions of hightemperature creep increases signiﬁcantly. If a cyclic heat treatment involves a phase transition within its temperature range of thermal cycling (e.g., the α ↔ γ transformation in iron and its alloys), the structural changes of a cyclic heat treatment arise as a result of both the plastic deformation caused by thermal stresses and the phase transitions. At low rates of heating and cooling (or for a small difference between Tmax and Tmin ) phase transitions play the main role, and the presence of these transitions can result in the production of tiny uniform sized grains which increase the plasticity and strength of the material. CYCLIC STRENGTH

Resistance to fatigue failure of materials under the application of cyclic loads. Quantitatively cyclic strength may be estimated by the endurance limit. As a rule, cyclic strength is somewhat lower than static strength. First of all, cyclic strength is determined by the maximum cyclic stress and its

amplitude. The greater the average cyclic stress, the lesser the stress amplitude needed for material destruction at the same test base. The character of the stress change between σmax and σmin has a negligible effect on the cyclic strength. That is why cycles of complicated shapes may always be reduced to ordinary ones, and standard fatigue tests are carried out with the use of the simplest cycle conﬁguration. An increase of the cycle frequency, other things being equal, usually gives rise to an increase in the cyclic strength, especially at high temperatures. So long as fatigue cracks are forming from regions of stress concentration on the surface, their state strongly inﬂuences the resulting cyclic strength. As the temperature increases, a shift of fatigue curves towards lower stresses is observed. When temperature changes take place, fatigue disturbances may also arise because of the onset of thermal stresses. Cyclic strength rises with the increase of metal purity with respect to interstitial elements, with the decrease of grain size, and with the formation of a cellular dislocation structure (see Fragmentation). It also depends on the presence and size of the second phase of dispersed particles. The environment in contact with the surface of the crack affects the crack growth due to physicochemical processes taking place at its peak (see Fatigue crack growth). The reliable determination of the cyclic strength is only possible when one takes into account the nature of the product, and the details of the fatigue. CYCLOTRON FREQUENCY, gyromagnetic frequency

Gyromagnetic frequency Ω of charged particle rotation in a constant magnetic ﬁeld B in a plane perpendicular to the ﬁeld. For a free charged particle the cyclotron frequency Ω is determined from the balance of the Lorentz force ev × B by the centrifugal force mv 2 /r, and it is given by Ω = eB/m, where e and m are, respectively, the charge and mass of the free particle, and v = Ωr. The cyclotron frequency determines the energy difference E between the energy levels of a particle in a magnetic ﬁeld: E = Ω. In crystals the motion of particles is more complicated since they interact with the ions of the lattice. In a constant

CYCLOTRON–PHONON RESONANCE

magnetic ﬁeld the energy of the electron (or hole) E and the projection pB of its quasi-momentum p along the direction B are conserved. Hence in momentum space the motion takes place along the intersection of the isoenergetic surface E(p) = E with the plane pB = const. If this curve is closed then the motion is periodic with the frequency Ω = eB/m∗ , where m∗ is the charge carrier cyclotron effective mass. CYCLOTRON PARAMETRIC RESONANCE

Selective absorption of electromagnetic radiation by a semiconductor located at the maximum magnetic ﬁeld of a stationary wave (frequency ω) inside a resonator, when a longitudinal constant magnetic ﬁeld B0 is applied, and the cyclotron frequency Ω is a multiple of half the pump wave frequency ω. Cyclotron parametric resonance is due to instability, arising from time modulation of the electron cyclotron rotation frequency (see Cyclotron resonance). The stabilization of this instability results from nonlinear processes, arising at large electron energies, that lead to a highly nonequilibrium and anisotropic distribution of carriers formed at the cyclotron parametric resonance. The presence of this distribution results in the generation and ampliﬁcation of electromagnetic and acoustic vibrations in semiconductors over a broad frequency range. In a thin sample at cyclotron parametric resonance the electron distribution function is independent of the coordinates. In a bulk semiconductor, when the sample size exceeds the wavelength of the pumping wave in the resonator; then the heterogeneity of the wave magnetic ﬁeld plays an important role. The emerging nonequilibrium distribution becomes rather heterogeneous. It results in gradients of the average energy and concentration, and ﬁnally it gives rise to a static electric ﬁeld Eind (hence a static electromotive force) and a heterogeneous Hall effect with a resonance character. The main cyclotron parametric resonance appears when the cyclotron frequency Ω0 = eB0 /m (e and m are particle charge and mass) is half the modulation frequency ω/2 (Ω0 ∼ ω/2 for linear polarization of the pump ﬁeld in a rectangular resonator, and Ω0 ∼ ω for circular polarization). Cyclotron parametric resonance, like any other parametric resonance of mechanical or electrical vibrations, occurs in resonance zones of instability, and diminishes with the

271

increase of the resonance number n (Ω = nω/2, n = 1, 2, 3, . . .). This resonance can be observed when the electrons make many revolutions in B0 before they collide with other particles and scatter, i.e. Ω0 νl , where νl is the a relaxation rate of the electron pulse. In solids collisions of the conduction electrons with crystal lattice defects (νl = 109 –1011 s−1 ), and scattering by thermal vibrations (electron–phonon interaction) are the most important. The last process limits the observation region of cyclotron parametric resonance: it is at low temperatures (1 to 10 K), where collisions with thermal phonons become rather infrequent. The actually achieved relaxation times provide the lower limit of the frequency region (ω > 109 Hz) where cyclotron parametric resonance can be detected at the ﬁeld value B0 = 0.1 to 1 T. This resonance is a threshold-type effect which can be observed when the pump levels are rather high, i.e. Ω1 > (νe νl )1/2 , Ω1 = eB1 /m, where B1 is the amplitude of the alternating magnetic ﬁeld, and νe is the relaxation rate of the electron energy, νe ≈ (10−4 –10−3 )νl . This condition is valid in ﬁelds B1 ∼ 0.01–0.1 mT. The energy of the resonance particles increases exponentially with time, and can attain large values (electron gas overheating can reach 100 K). It results from the fact that the electron distribution becomes rather nonequilibrium and anisotropic. The energy increase is not inﬁnite, but is limited by nonlinear processes. These are processes such as the nonquadratic spectrum of conduction electrons, which results in the dependence of the mass (and the cyclotron frequency) on the energy, and also affects the energy dependence of the electron relaxation rates. Cyclotron parametric resonance can be used as a method of high-frequency resonance pumping of electrons in conductors to produce an inverted population distribution of charge carrier energies. CYCLOTRON–PHONON RESONANCE

A sharp increase of the electromagnetic wave absorption in semiconductors, when the condition ω = ω0 + nωL is satisﬁed, where ω is the electromagnetic wave frequency, ω0 is the optical phonon frequency, ωL is the Larmor precession frequency, and n is an integer. The resonance is observed at high frequencies (ωτ 1) and in a quantizing magnetic eld (ωL τ 1, ωL kB T ); τ is the

272

CYCLOTRON RESONANCE

time of the electron mean free path. The resonance is associated with transitions of electrons between Landau levels with the simultaneous absorption of a photon and an optical phonon. The singularity of the absorption coefﬁcient at its approach to resonance has a logarithmic nature. Cyclotron–phonon resonance has often been studied experimentally. It is used to determine semiconductor parameters, and in particular the frequency of the optical phonon.

on the Luttinger Hamiltonian matrix. In addition to cyclotron resonance there are spin resonances of free carriers (combined resonance and paramagnetic resonance). These types of absorption, together with the investigation of magnetooptical interband transitions, provide a reliable starting point for understanding energy band structures (see Band theory). CYCLOTRON RESONANCE, ACOUSTIC See Acoustic cyclotron resonance.

CYCLOTRON RESONANCE

Resonant absorption of radiofrequency or microwave energy by an electron or other charged particle in a static magnetic ﬁeld when its gyrofrequency equals the frequency of a perpendicular electric ﬁeld. It corresponds to the diamagnetic resonance absorption of an electromagnetic wave, accompanied by the transition of an electron (or hole) from one stationary orbit to another (mainly, to a neighboring one) in a crystal situated in an external constant magnetic ﬁeld B. By its nature this is an electric dipole resonance. In a solid a charge carrier can move freely longitudinally along B. The transverse motion takes place in a ﬁxed orbit with energy equal to ωc n (in an elementary Brillouin zone with energy E(k) = 2 k 2 /(2m∗ )), where ωc = eB/m∗ is the cyclotron frequency and n is a positive integer (Landau levels). In the case of absorption, the change of carrier energy is ωc for the ground state absorption, and a multiple of ωc for harmonics arising when the dependence E(k) is more complex. The nature of E(k) can be deduced by methods of group theory in solid state physics. A main feature of cyclotron resonance is the possibility of determining the effective mass m∗ directly through a measurement of the absorption frequency. When E(k) is anisotropic then ωc depends on the angle between B and the symmetry axes of the crystal. The main condition for observing cyclotron resonance is the requirement that the conduction electron be able to complete an orbit before colliding (ωτ > 1), where impurities, heterogeneities, and crystal lattice vibrations determine the scattering time τ . For complicated forms of the energy E(k), in particular for the presence of both light and heavy holes in cubic semiconductors, the equations of motion have an obvious classical interpretation. The theory uses a quantum-mechanical calculation based

CYCLOTRON RESONANCE IN METALS, Azbel–Kaner resonance In metals cyclotron resonance amounts to an increase in the high-frequency conductance at fre-

quencies ω which are multiples of the electron cyclotron resonance frequency in a constant magnetic ﬁeld parallel to the sample surface. This phenomenon is due to the repeated synchronous acceleration of electrons during the part of the orbit located within the skin depth δ (see Skineffect). In 1956 M.Ya. Azbel and E.A. Kaner theoretically predicted cyclotron resonance in metals, and E. Fawcett discovered it in Sn and Cu. It has been observed in over 32 metals. The electron acceleration mechanism for cyclotron resonance in metals is as follows (see Fig.). For a magnetic ﬁeld B parallel to the metal surface all electrons move in circular orbits, and periodically with the cyclotron frequency Ω they return to and pass through the skin δ where they are accelerated by the electromagnetic wave. If the resonance condition ω = nΩ, n = 1, 2, 3, . . . , is satisﬁed then the acceleration of the electrons takes place on each cycle of the trajectory, just as it occurs in a cyclotron with a single accelerating region. The skin depth δ in a metal plays the role of the latter. The metal region outside the skin acts as the dees

Cyclotron resonance in metals.

CYCLOTRON WAVES

of the cyclotron. Cyclotron resonance is observed in pure single crystal metals at helium temperatures when the rate of electron collisions is less than Ω. It is observed only for the conditions of the anomalous skin-effect, when the radius of the orbit R and the electron mean free path l are much larger than the skin depth δ. Cyclotron resonance in metals differs significantly from diamagnetic cyclotron resonance in semiconductors. The latter is also called cyclotron resonance when it takes place in a gas-discharge plasma. Diamagnetic resonance occurs in a homogeneous radio-wave ﬁeld. Therefore: (a) it is observed at the fundamental frequency (ﬁrst harmonic) ω = Ω, but not at multiple frequencies, as is the case of cyclotron resonance in metals; (b) it is a maximum when the polarization of the rf electric ﬁeld is perpendicular to the vector B, whereas cyclotron resonance in metals exists at any polarization; (c) it is characterized by a sharp increase of the electromagnetic absorption at resonance, while absorption decreases at cyclotron resonance in metals. The last circumstance is associated with the fact that a sharp increase of the current at cyclotron resonance in metals results in its resonance screening from the the external wave, in the increase of the reﬂection coefﬁcient, and, therefore, in a decrease of the energy absorption. The line shape of cyclotron resonance in metals is rather asymmetric due to the presence of intrinsic cyclotron waves, which have their spectrum localized near harmonics nΩ of cyclotron frequencies. In the case of a nonquadratic electron dispersion law, which is typical for most metals, the cyclotron frequency Ω depends on the value of the electron momentum projection along the direction B, hence it differs for different electrons. In this case cyclotron resonance in metals occurs at the extreme frequencies nΩext , since for electrons with Ωext there is a singularity in the density of states. Owing to the decrease of the resonance electron number the amplitude of the cyclotron resonance in metals decreases, and the lines broaden and become more asymmetric in comparison with the case Ω = const. In so doing the resonance of electrons from the central cross-section, and from the vicinity of special points of the Fermi surface, becomes sensitive to the wave polarization. A small slope of the ﬁeld B relative to the surface leads

273

ﬁrstly to the splitting of the resonance peaks, then to the doubling of their number (Ω = nΩ/2), and to the inversion of the lines. In numerous experiments on cyclotron resonance in metals an important fact has been established: electron scattering on the surface heterogeneities of the sample is almost of the mirror-type. It results in a considerable decrease of the amplitude of the cyclotron resonance in metals, since there arises a new group of electrons sliding along the surface near the mirror boundary of the skin depth. Their contribution to the current is rather more than the contribution of resonance particles, and cyclotron resonance in metals arises from corrections to the smooth nonresonance part of the surface impedance of metals. A complete self-consistent theory of cyclotron resonance in metals at arbitrary reﬂections of electrons from the metal surface over a wide range of frequencies and magnetic ﬁelds has been developed. CYCLOTRON RESONANCE, QUANTUM See Quantum cyclotron resonance. CYCLOTRON WAVES

Intrinsic electromagnetic excitations of degenerate electron–hole solid-state plasmas in a magnetic ﬁeld B. The spectrum of cyclotron waves is localized near the cyclotron resonance frequencies ω = nΩ (n = 1, 2, 3, . . .), for a wave vector k⊥B. Its origin is the collective precession of electrons with the cyclotron frequency Ω, in the absence of magnetic collision-free damping. The distinguishing features of this spectrum are due to the nonlocal properties of the conductivity operator, and depend on the electron dispersion law. For the square law of dispersion there are three independent waves in the vicinity of each cyclotron resonance, namely the ordinary, extraordinary, and longitudinal ones, differing in their spectrum and polarization. The spectrum of the transverse cyclotron waves begins at the point k = 0 from the frequency nΩ, reaches a minimum (about nΩ − Ω/2) at k ∼ R −1 (R is the cyclotron radius), and then asymptotically approaches the initial value nΩ. The attenuation of cyclotron waves is determined by the rate of electron relaxation. Parameters of the Fermi liquid interaction in alkali halides have been measured by cyclotron waves.

This Page Intentionally Left Blank

Dd with different orientation in a unit cell. It is observable by the splitting of bands of absorption and luminescence, the components of which appear to be polarized in orthogonal directions. Davydov splitting happens in the spectra of inorganic crystals with ionic or mixed-type bonds in which one can distinguish groups of strongly bound atoms with different orientation in the lattice (K2 CrO4 , CaWO4 , etc.). Davydov splitting is especially apparent in semiconductors with a layered and chain-like structure (As2 S3 , CdP2 , ZnP2 , etc.) where the unit cell is composed of atoms belonging to two or more translationally inequivalent chains or layers, between which, like in molecular crystals, there is a weak van der Waals bond (see also Fermi–Davydov combined resonance, Van der Waals forces). Davydov splitting in liquid crystals is close in nature to Davydov splitting in crystals with several molecules in the unit cell and is of the order of νe ∼ 10−13 s−1 for electronic transitions or

νv ∼ 10−11 s−1 for vibrational transitions. In liquid crystals, there appears an additional contribution to the splitting, which is associated with the orientation dependence of the dispersion interaction. It is comparable in its magnitude with the Davydov splitting, and observable in impurity absorption bands.

DAMPING, COLLISION-FREE See Magnetic collision-free damping. DAMPING, LANDAU See Landau damping. DANGLING BOND, broken bond An unsaturated covalent bond; a bond from

one atom without a terminus, a kind of structural defect in a solid involving a covalent or ioniccovalent bond. Broken bonds are inherent in both crystalline and amorphous solids (see Amorphous state), and can be arranged in a type of random continuous network; this is common in organic and polymeric glasses (see Vitreous state of matter). Associated with broken bonds in amorphous semiconductors and insulators are features of the electronic spectrum that signiﬁcantly affect the processes of electron transfer and photostimulated phenomena. In many cases broken bonds sufﬁciently high in concentration can be observed with the help of electron paramagnetic resonance since they involve unpaired electrons. The density of broken bonds in amorphous solids can reach 1020 to 1021 cm−3 . Examples of broken bonds are unsaturated bonds of surface atoms. Since the energy can be lowered by saturation (closure) of broken bonds, efforts are made toward surface reconstruction of covalent crystals, and this is an important factor in chemisorption on crystals.

DE BOER PARAMETER (J. de Boer, 1948)

DAVYDOV SPLITTING (A.S. Davydov, 1948)

Ratio of the amplitude of the zero-point vibrations of the atoms in a crystal to the crystal lattice

Splitting of electronic, electronic-vibrational and vibrational states in molecular crystals caused by the presence of inductive coupling between molecules and by the migration of excitation energy in a crystal. Davydov splitting is possible when there are two or more identical molecules

spacing, denoted by ΛB . This provides the stability criterion of the classical crystal state, namely, ΛB 1. However, there are crystals for which ΛB ∼ 1. Since the existence of the crystalline state in such a situation is itself problematic, the deﬁnition of the de Boer parameter should not contain 275

276

DE BROGLIE WAVE

the lattice period. It is determined through the parameters of the pairwise interaction of atoms, parameters of the Lennard-Jones potential. The de Boer parameter for a series of elements has the values: 3 He

4 He

H2 D2 Ne Ar K Xe 0.48 0.43 0.28 0.20 0.09 0.03 0.02 0.01 Crystals for which ΛB ∼ 1 are called quantum crystals. DE BROGLIE WAVE (L. de Broglie, 1924)

The quantum mechanical attribution of wave properties to microparticles (electrons, atoms, molecules, etc.). According to the assumption of L. de Broglie a moving particle with the energy E and momentum p has associated with it a wave with a frequency ν = E/ h and a wavelength λ = h/p. The de Broglie wave length corresponding to the thermal motion of the particles increases with the decrease in temperature T . At a sufﬁciently low temperature when λ becomes comparable to the distance between the particles of a system, then quantum effects begin to play a role (see Quantum liquid, Quantum crystal). DEBYE FREQUENCY See Speci c heat. DEBYE–HÜCKEL THEORY (P. Debye, E. Hückel, 1923)

Thermodynamic theory of electrolytes taking into account the screening of the electrostatic potential (see Electric charge screening) by the mobile ions of the solution. It follows from Debye– Hückel theory that an ion located within the solution is surrounded by a coordination sphere of ions of opposite sign, its radius being l D = # εkB T /(8πe2 I ), where ε is the dielectric constant, I is “ionic force” of the solution, I = (1/2) i ni Zi2 where ni is the concentration of ions of the ith type, and Zi is the valence of the ith ion. The coefﬁcient of activity of the ith ion is equal to exp[−Z+ Z− e2 /(2k B T εl D )], where Z+ , Z− are valences of ions of the corresponding sign of the charge. In the Debye–Hückel theory the possibility of forming a bound pair of oppositely charged ions is also taken into account (in this

case the components of the pair provide the mutual screening). The relation between the concentration of pairs and the concentration of individual screened ions is determined by the total concentration of ions in the solution. This theory is used for the description of defects in nonmetallic crystals, e.g., for the calculation of diffusion coef cients, of ionic conductivity, etc. DEBYE–SCHERRER METHOD, powder X-ray method, polycrystal method (P. Debye, P. Scherrer)

Method of obtaining the diffraction diagram of a polycrystalline material (see Polycrystal) by X-ray scattering. In this method a monochromatic narrow beam of X-rays is incident on a sample in the form of a cylinder or a polished section from a polycrystal. All the crystallites in the sample are assumed to have random spatial orientations, and the Bragg condition is satisﬁed for each set of suitably oriented crystallographic planes. For each allowed crystallite orientation diffracted X-rays will emerge along a cone coaxial with the incident X-ray beam with an aperture angle 4θ , where θ is a Bragg angle (see Bragg law). The result is a family of cones corresponding to diffracted X-rays with various allowed aperture angles 4θ for the various allowed reﬂections. The diffraction picture in the Debye–Scherrer method may be recorded on a cylindrical or ﬂat photographic ﬁlm (debyegram). In the X-ray diffractometry of polycrystalline samples the photographic ﬁlm is replaced by a rotating detector of X-rays. DEBYE TEMPERATURE (P. Debye, 1912) The characteristic crystal temperature Θ D cor-

responding to the Debye frequency ωD (k B Θ D = ωD ), where ωD is the maximum frequency of the crystal lattice vibrations of the crystal (ωD ∝ vs /a, where vs is the sound velocity and a is the crystal lattice constant). In the Debye model the crystal vibration frequencies ω are limited by the Debye frequency (ω ωD ), and the linear dispersion law ω = vs |k| is assumed to be valid, where k is the phonon wave vector which takes on 3N discrete values (N is the number of atoms in the crystal), the largest value of k being π/a. The numerical values of the Debye temperature depend on the atomic mass, and on the strength of the elastic bond between atoms (e.g., for Pb Θ D ∼ 90 K,

DECHANNELING

for diamond Θ D ∼ 2340 K). Knowledge of the value of Θ D allows one to obtain important information about the vibrational spectra of a crystal, and about the characteristics of its chemical bonds. The notion of a Debye temperature is essential for treating the thermodynamics of crystal; it is the approximate temperature boundary which separates the low-temperature (T Θ D ) and high-temperature (T Θ D ) lattice properties of the crystal, where T is the crystal temperature. Using only the single parameter Θ D together with some approximation expressions it is possible to describe the behavior of a whole series of observed physical characteristics of crystals over a broad temperature range below as well as above the Debye temperature. Examples of these are: speci c heat, electrical resistance (Bloch–Grüneisen formula), elastic moduli, Debye–Waller factor for the scattering of X-rays, neutrons, electrons, etc.; properties involving the Mössbauer effect, IR absorption, etc. DEBYE THEORY OF SPECIFIC HEAT See Speci c heat. DEBYE–WALLER FACTOR (P. Debye, I. Waller)

The temperature factor in the expression for the probability of the radiation of photons from crystals, or of elastic processes for the scattering of particles or photons, which takes into account thermal and static displacements of atoms from their sites on a crystal lattice. The Debye– Waller factor is written in the form e−2W , where e−W = exp[iQ(uth + ust )], . . . means double (thermodynamic and conﬁgurational) averaging, and Q is the scattering vector or the wave vector of the radiated photons. If the displacements are counted with respect to the sites of the “average” lattice, W assumes the approximate form W ≈ (1/2)[Q(uth + ust )]2 . In the isotropic approximation 2Wα = (Q2 /3)u2α . For a monatomic crystal, assuming the Debye model, it has the temperature dependence 3Q2 2π 2 T 2 1+ + ··· , 2Wth = 8MkB ΘD 3 ΘD where Θ D is Debye temperature, and T is absolute temperature of the crystal. In the general case Wth . depends on the force constants of the

277

crystal, on the atomic masses and on temperature. The static Debye–Waller factor depends on the elastic constants of the crystal, and on the characteristics of defects (concentration, dimensions, correlation in their location, etc.). Usually Wth 1, and for room temperature W th ∼ 0.01 to 0.1. For impurity atoms, small clusters and dislocation loops W st 1; for dislocations W st 1 and the effects of coherent dissipation disappear in the kinematic approximation; but taking into account the dynamic effects of scattering W st in the case of dislocations requires renormalizing, while, e.g., for the scattering of X-rays the renormalized Debye–Waller factor W st < 1 for a dislocation density less than 105 to 107 cm−3 . The Debye–Waller factor determines the reduction of the coherent scattering intensity I (Q) of X-rays, neutrons and other radiations in crystals: I (Q) = I0 (Q) e−2W , where I0 is the intensity of scattering by the ﬁxed ideal (average) lattice. A Debye–Waller factor also describes the efﬁciency of gamma ray radiation in a crystal without recoil (see Mössbauer effect); in this case it is sometimes called the Lamb–Mössbauer factor. DECA. . . (fr. Gr. δεκα , ten), da

Decimal preﬁx which denotes a 10-fold increase of the value of the basic unit. For instance, 1 dal (dekaliter) = 10 l. DECAY, ISOSTRUCTURAL See Isostructural decay. DECHANNELING Exit from the channelling mode; inﬂuenced by the excitation of phonons, electrons, plasmons,

etc., by the channeling particles. Motion of the channeled particles in the transverse direction can be considered as a drift in the ﬁeld of a random force, caused by deviations from the average continuous potential. In this case the energy of the transverse motion of the channelized ions E⊥ increases in proportion with their movement along the channels (upon reduction of their total kinetic energy), and upon reaching the critical value E⊥c = E0 Ψk the dechanneling occurs; E0 is the initial channelized particle energy, Ψk is the Lindhard angle (see Channeling). The distance at which the density of channeling particles

278

DECI. . .

is reduced by one half is called the dechanneling length. This length for protons with energies from 1 to 10 MeV in silicon lies within the range from 2 to 18 μm. Dechanneling is enhanced by the presence of defects in crystals, especially by impurity or inherent interstitial atoms, located near the axes of the channels, and also by dislocations; in alloys it depends on the degree of ordering, etc. DECI. . . (fr. Lat. decem, ten), d

The decimal fraction preﬁx meaning 1/10 of a particular unit. For instance, 1 dg (decigram) = 0.1 g. DECOMPOSITION OF ALLOYS See Alloy decomposition. DECOMPOSITION, SPINODAL See Spinodal decomposition. DECORATION See Surface decoration. DEEP ENERGY LEVELS AND GREEN’S FUNCTIONS See Green’s functions and deep energy levels. DEEP LEVELS in semiconductors Local electronic levels in semiconductors whose ionization energies are comparable with the band gap width. Deep levels exhibit a diversity of prop-

erties due to their depth, and their physicochemical characteristics. The atoms Zn, Cd, Mn, Fe, Co, and Ni in Si and Ge are double (M2+ ) acceptors; Cu and Ag are triple acceptors, and the impurity Au in Ge produces three acceptor and one donor level. Deep levels are responsible for a series of special electric, optical, photoelectric and other properties in semiconductor materials. The direct introduction of impurities is the main method for obtaining material with the desired properties. Deep level centers possess abnormally large cross-sections for trapping of current carriers, so they can serve as centers of rapid recombination. An attempt to formulate a quantitative theory of deep levels encounters some signiﬁcant obstacles associated with the need for a microscopic description of the defect portion of the crystal and with the multi-electron nature of the problem (i.e. simultaneously taking into account both

the electrons of the defects and the valence electrons of neighboring atoms). For calculating local level parameters given in the literature, various quantum chemical methods are used (see Quantum chemistry of solids), in particular, a Lifshits method of regular perturbations (Green’s functions), a modiﬁed method of effective mass, and some others. These methods are arbitrary in their choice of the periodic ﬁeld potential perturbed by a defect in an ideal crystal, and as a rule are not very accurate. DEFECT

For different varieties see Defects in crystals, Defects in liquid crystals, Anti-Schottky defect, Antisite defect, Antistructural defect, Electrically active extended defects, Frenkel defect, Grainboundary defects, Intrinsic defects, Macroscopic defects, Monopole-type defect, Needle-shaped defect, Planar defect, Rod-shaped defects, Schottky defect, Stacking faults, Stoichiometric defects, Surface defects, Swirl defects, Thermal defects. DEFECT CLUSTERING See Point defect clustering. DEFECT ELASTIC POTENTIAL See Elastic potential of a defect. DEFECT INTERACTION See Elastic interaction of defects, Strain interaction of defects. DEFECTON A quasi-particle which arises from a light defect of a crystal lattice as a result of quantum tunneling (see Tunneling phenomena) through the periodic relief of a crystal. A defecton is characterized by a quasi-momentum which determines its

energy, usually lying within a narrow allowed energy band (defecton band). A vacancion (vacancy wave) in solid helium and an impurity atom of 3 He in crystalline 4 He (impuriton) exemplify defectons. Defectons take part in quantum diffusion which has an unusual temperature dependence, and is very sensitive to the concentration of defects. Due to the small width of the defecton band a non-uniform strain of a crystal brings about the localization of defectons, and their transformation into ordinary point defects.

DEFECTOSCOPY

DEFECTOSCOPY, aw detection

The totality of methods which permit the detection of defects (cracks, pores, gas blisters, extraneous inclusions, liquation, segregation of impurities, etc.) in the structure of a solid. There are several types of defectoscopy. Magnetic defectoscopy records the spreading out of magnetic ﬁelds in the regions of defects, or measures the magnetic properties which change in the presence of defects in the material (ferromagnetic materials or ferromagnetic inclusions in nonmagnetic materials). There are the following variants of magnetic defectoscopy: magnetic-powder method where the scattering ﬁelds are detected at the surface of a magnetized sample of small (several μm) particles of ferromagnetic powders or suspensions (recording is visual); the magneticluminescent method where luminofores are used as powder (particle location recorded using UV radiation); the magnetographic method uses superposition at a ferromagnetic ﬁlm, which is then studied with the aid of a tape-recorder head and an electron-beam indicator; the ferroprobe method using different ferroprobes (in particular, taperecorder heads, magnetic diodes, induction coils, etc.) for recording the scattering ﬁelds. Electrical defectoscopy records the spreading out of the electric ﬁelds near defects, thermal electromotive force, electrical resistance. X-ray defectoscopy detects defects by the variation of the contrast from X-rays passing through the sample. This is applicable to thick samples, and uses photographic ﬁlm or special sensors which record the X-ray intensity at every point of the space, subject it to analysis, and transmit the results to a video device screen. Gamma defectoscopy uses the variation of the intensity of gamma rays passing through the material in the region of defects, and is applicable to thick samples. Beams of high-energy electrons generated by accelerators can detect hidden defects in critical materials. Neutrons can detect defects in massive structures and engineering devices, as well as the concentration of inhomogeneities in ordinary bodies. Defectoscopy based on dynamic light scattering in nematic liquid crystals is used for the

279

control of insulating layers on metal–insulator– semiconductor structures (integrated circuits, conductive plates with dielectric coating, etc.). This method can detect 1 μm pores in insulators, and it provides a nondestructive control of a structure with dielectric insulation, giving information about the type of defects present. The most widespread use of acoustic defectoscopy is the shadow method where the reduction in amplitude or the variation of phase of the incident wave, scattered by the acoustic non-uniformity, is recorded, and the echo-method which measures the time of return of a short acoustic pulse to the piezo-transformer after reﬂection from a defect (see Piezoelectricity). The minimum dimensions of recorded defects and the accuracy of their localization by these methods is of the order of the ultrasound wave length. Also there is a series of special methods for measuring speciﬁc parameters of samples. For instance, the thickness of plates is controlled by the value of their resonance acoustic frequencies, the quality of lamellar structures by their acoustic impedance, and the presence of defects in strongly sound-adsorbing bodies through the spectrum of their free (low-frequency) oscillations. Physico-chemical methods of investigation include the capillary method, luminescent analysis, the chromatic method which employs the interaction of surface-active liquids (see Surfaceactive agents) with defects located at the surface or in regions close to the surface. To investigate microdefects of the structure, the method of etching with subsequent microscopic or electronmicroscope analysis is used (see Electron microscope). Upon the interaction of the crystal surface with a chemically-active medium the points of exposure of the defects, e.g., of dislocations, are “etched” more intensely, and this is then detected by optical or scanning electron microscopy. Dislocations and dislocation loops in foils are detected by transmission electron microscopy. Electron– positron annihilation (see Positron spectroscopy) detects and identiﬁes microdefects due to the ability of positrons to localize and annihilate in the defective areas of the crystal. The processing of positron annihilation spectra or the analysis of their lifetime gives information about the type and distribution of microdefects in crystals. The use of

280

DEFECT RESISTANCE

different types of penetrating radiations and their transformation into optically visible images with the help of special electronic devices called image transformers is a type of defectoscopy. X-rays, γ -quanta, β-radiation of isotopes, beams of highenergy electrons and ions, neutrons, electromagnetic radiation in the range from the near infrared to millimeter and submillimeter waves, are used as penetrating radiations (see Optical defectoscopy). DEFECT RESISTANCE

A property of a material whereby it resists damage and possible failure through the effect of small concentrators of stresses (see Stress concentration). Examples are scratches, small cracks, rough nonmetallic inclusions and other defects, which are fractions of a millimeter in size, i.e. no more than 1 or 2 orders of magnitude larger than the size of a polycrystalline metal grain (see Polycrystal). The defect resistance parameter is a quantitative measure of the defect resistance: D2 = log K v − nτ where K v = R ms /στ is the viscosity coefﬁcient of the metal, R ms is the microspalling resistance, στ is the yield limit, and nτ is the exponent in the parabolic equation governing the initial stage of strain hardening of the metal, σe = Aen (A is a constant, e is the actual strain or deformation): nτ =

log(S v /στ ) , log(ee /eτ )

where S v is the true ultimate strength, ee is the uniform true strain, and eτ is the strain at the yield limit. The criterion of defect resistance D2 = log(σ1 /σi ) (where the ratio σ1 /σi is the rigidity of the state of stress at the vertex of the defect, σ1 is the main normal stress, σi is the intensity of stresses) expresses the condition for the destruction of a metal containing a small defect within an area of low plastic deformation of the magnitude e ≈ 0.02. The parameter of defect resistance as a characteristic of steel toughness supplements the index of fracture toughness (crack resistance), because the latter is not applicable to cracks and defects of submillimeter size. DEFECTS, CONTINUUM THEORY See Continuum theory of defects.

DEFECTS, HEALING See Healing of defects. DEFECTS IN CRYSTALS

Disturbances of the periodicity of atom (ion) positions within a crystal (structural defects). They are subdivided into point, linear, surface (or planar) and bulk types. Point defects are one dimensional imperfections (of atomic scale size) distributed in three dimensions. Examples are vacancies, interstitial atoms and some of their combinations (bivacancies, complexes, etc.), as well as impurity atoms which may be located at regular sites of the crystal lattice (substitutional atom) or between regular sites (doping atom). Unlike other types, point defects can be in thermodynamic equilibrium at the lattice temperature. Linear defects are small in two dimensions, and can have a considerable length in the third. The character of linear defects, and of the displacement ﬁelds created by them, is described by the Burgers contour. This contour may either close on itself or be open, and if it is open then the Bravais lattice vector connecting the starting and ending points is called the Burgers vector. Needleshaped defects characterized by a closed contour are chains of vacancies or interstitial atoms. They are not very stable, and easily decompose by thermally activated or tunnel diffusion of atoms. Dislocations correspond to open Burgers contours. Lattice disturbances which are elongated in two dimensions and small in the third are called surface defects. They form at crystal locations where adjoining lattices differ from one another by space orientation or by atom positionings. Some characteristic types are stacking faults, grain boundaries, and subgrain boundaries (see Subboundaries). Bulk defects are disturbances which are not small in any of their three dimensions. Aggregates of point defects, pores and inclusions of a second phase are included in this type. The inﬂuence of defects on the physical properties of crystals is extremely diverse. It is determined by the character of the binding forces within the crystal, by their energy spectrum (metals, semiconductors, insulators), by the nature of the defects, etc. In semiconductors and insulators, where good electrical, optical or photoelec-

DEFECTS IN PHASE TRANSITIONS

281

tric properties are crucial (see Photoelectric phenomena) point defects play an important role, and dislocations may also make a considerable contribution to the electrical resistance. In construction materials where high strength is essential (see Strength), the role of surface and bulk defects is important. An atmosphere of point defects can strongly inﬂuence the motion of dislocations (see Cottrell atmosphere).

Defects in liquid crystals.

DEFECTS IN LIQUID CRYSTALS

Inhomogeneities of the orientational (see Orientational order) and/or translational ordering of molecules of liquid crystals. Molecular size and macroscopic defects are distinguished. Those of molecular size are formed by additions into the liquid crystal, e.g., molecules of dyes, of ions, of surface-active agents, or as a result of lightor radiation-induced transformations of molecules already present. Macroscopic defects include the following: point defects (hedgehogs, boojums), linear ones (dislocations, linear solitons), planar defects (domain walls) and bulk defects (particlelike solitons). Macroscopic defects are called topologically stable if no continuous transformation is able to transform the ﬁeld of the order parameter to the uniform state. The classiﬁcation of macroscopic defects is based on the calculation of the homotopic groups πi (R) of the space of rank R (region of degenerate states) of the medium. Each class of defects corresponds to an element of the group, identical within the accuracy of continuous transformations of the order parameter; a state without a defect corresponds to the unit defect. This formalism permits one to associate with each class of defects some topological invariant, called the topological charge, which is a generalization of the Burgers vector in the theory of dislocations. The continuous variation of the topological charge of an isolated defect is impossible. In the general case the homotopic group πi (R) classiﬁes a defect of dimensionality d = d − i − 1, where d is the dimensionality of the medium. In a three-dimensional (d = 3) medium group π0 (R) describes walls (i = 0, d = 2), π1 (R) describes lines (d = 1), and π2 (R) describes points (d = 0). The processes of decomposition and merging of the defects are limited by the multiplication law of the group elements. If the group is

Abelian (all elements commute) the result of such processes is always unambiguous, while for a nonAbelian group the result depends on the path along which the decomposition (merging) of the defects occurs. Macroscopic defects cause distortions of the orientation of liquid crystal molecules within the whole volume of the sample. Since it is the orientation of the molecules which determines the distribution of the optical axes (see Director) of the liquid crystal, the defects are easily subjected to investigation by the methods of polarization microscopy (see Optical polarization method). The formation and motion of defects play important roles in practically all processes of the liquid crystal response to external disturbances, such as the stress relaxation, the reconstruction of structure under the effect of an electromagnetic ﬁeld, at phase transitions, etc. As a rule, some topological defects are present even in the equilibrium state of a liquid crystal, and their stability is provided by the boundary conditions (see Fig.). Thus, for example, in a spherical drop of a nematic material (see Nematic liquid crystal) with normal boundary conditions in equilibrium there always exists a point defect within the volume, the hedgehog (Fig., right), and at the tangential lines there are two boojums or surface point defects (Fig., left). Due to the wide variety of defects, and the possibility of performing a broad range of experiments, defects constitute convenient models for the development of topological representations in condensed matter physics (see Topological inhomogeneity). DEFECTS IN PHASE TRANSITIONS

Phase transition defects are of two types, those involving a random local ﬁeld, and those involving

282

DEFECT STRESS SCALE

a random local temperature, depending on their inﬂuence upon the coefﬁcients of the density η(r) or the thermodynamic potential Φ(r) describing the phase transition. Within the phenomenology of the Landau theory, the density in the absence of defects has the form: 2 B D A Φ(r) = η2 (r) + η4 (r) + · · · + ∇η(r) 2 4 2 + · · · − h0 η, (1) where for simplicity the long-range forces are not taken into account, and the one-component order parameter A = A0 (T −T0 ) is included; B, D, A0 are medium constants, and h0 is the external ﬁeld which is conjugated to the order parameter. Point defects of the random local ﬁeld type add the following contribution to Φ(r): hi (r − ri )η(r), (2)

Φh = i

and defects of the random local temperature type lead to the additional contribution 1

ΦT = A(r − ri )η2 (r). 2

(3)

The origin of the terms, defects of random local ﬁeld and random local temperature, is associated with the fact that the “averaged over conﬁguration” values Φ h (r) = hη(r), Φ T (r) = (1/2)Aη2 (r) describe renormalization by the defects of the value of the external ﬁeld h0 and of the phase transition temperature T0 . The local ﬁeld defects bring about strong local distortions of the crystal matrix, because it follows from Eq. (1) that (not too close to T0 ) η(r) ∝ (1/r) exp(−r/r c ) with r 2 c = D/A → ∞ at T → T0 . These defects eliminate the long-range order (see Long-range and short-range order), leading to a complex domain structure in systems with inﬁnitely degenerate η, or to long-term relaxation in systems with ﬁnite degenerate η. Such polarized defects create an average ﬁeld within the crystal, and induce η = 0 at any temperature T , i.e. the phase transition, speaking strictly, is absent (blurred). The random local ﬁeld defects bring about a shift of T0 and lead to anomalies of different physical values in the vicinity of T0 . In the area of similarity theory these defects cause a variation of the

critical indices. The reorienting random local ﬁeld defects are a special class of defects which, unlike frozen defects, bring about an increase in the temperature of pure crystal phase transitions. DEFECT STRESS SCALE See Stress scales of defect structures. DEFECT STRUCTURE ANALYSIS See Microprobe X-ray defect structure analysis. DEFECT SYMMETRY GROUP

This involves both the symmetry of a defect itself as well as the symmetry group of the crystal where the defect appears. Translational symmetry (see Translation) disappears when a single defect is introduced into a crystal. The point group of symmetry of a crystal with a defect reﬂects the symmetry of the point defect, and is a subgroup of the point group of the ideal crystal. If we disregard the crystal distortion induced by a defect then the symmetry of this defect is the same as the symmetry of the site that it occupies. The symmetry groups of the various points of the unit cells for all 230 space groups are given in the International Tables for Crystallography. For an impurity atom (or a vacancy) at a site of a Bravais lattice the defect point symmetry is the same as the crystal point symmetry. The presence of a pair of point defects, dislocation loops in cubic crystals, or particles of a new phase of different symmetry all result in a lowering of the symmetry compared with that of the host crystal. DEFECT THRESHOLD ENERGY See Threshold energy of defect formation. DEFORMATION AT LOW TEMPERATURES See Low-temperature deformation. DEFORMATION BY EXPLOSION See Explosion deformation. DEFORMATION DIAGRAM, stress–strain curve

Graphic representation of the dependence of the deforming force (stress) on the material response (strain). The deformation diagram reﬂects

DEGENERACY

the results of testing solids by different methods such as stretching, compressing, e xure and torsion. As deformation parameters one can select absolute values of elongation, of shearing angle, of torsion angle (see Rod twisting), of deﬂection, or preferably one can work with relative deformations which are ratios of sample dimensions during loading to those before the test. Relative deformations are usually subdivided into two types: a conditional deformation which is the the sum of successive variations of size all relative to the same initial dimension before the test; and a true deformation which is the sum of small variations of size, with each of them relative to the current value of the dimension. The deforming effort is characterized also by either the absolute value of the projection of the force or torsion along some direction (direction of deformation), or by the speciﬁc parameter of stress, i.e. by the force effecting a unit area of some cross-section of the body. The normal stress, namely the component of force perpendicular to the cross-section area, and the tangential stress, due to the projection of the force along (parallel to) the area of the cross-section, are singled out. The stresses are usually divided into conditional and true stresses: the former determined by the relation of the actual force to the initial area of the cross-section, and the latter by the same relation to the current area. To plot a deformation diagram it is possible to use different combinations of the above mentioned deformation and deforming force parameters. For the analysis of physical dependencies of the deformation process the diagram using the coordinates “true deformation–true stress” is the most signiﬁcant. This diagram provides data for the calculation of many basic mechanical parameters of the material (e.g., elastic moduli, yield limit, ultimate strength, strain hardening factor, margin of plasticity). The analysis of a deformation diagram also gives information about the physical mechanisms of plastic deformation, of hardening and of degeneracy. Alternate terminology for a deformation diagram is deformation curve, hardening curve and diagram of loading.

283

tion of temperature, strain, and rate of deformation. The simplest kinetic equation presenting a microscopic description of plastic deformation in terms of the dislocation model of plastic deformation takes the form: ε˙ = bρv, where ε˙ is the rate of deformation, b is the Burgers vector, ρ is the density of mobile dislocations, and v is the mean velocity of their motion. The deformation kinetics is accompanied by an irreversible displacement of dislocations. In addition to the displacement of dislocations, one has to consider the multiplication of dislocations and interactions between them, as well as the effects of other lattice defects, in particular, of disclinations. Two competing processes proceed simultaneously when a crystal is undergoing a deformation: strain hardening and recovery. During hardening the stresses required to maintain a constant rate of deformation increase, while the rate of deformation decreases, if a constant external stress is applied. Recovery decreases the rate of hardening during active deformation (˙ε = const), and produces a steady-state creep under a constant stress. Existing theories describe the deformation kinetics at the ﬁrst stages of deformation, in particular, the appearance of a yield cusp (upper and lower yield limits on the deformation diagram, or stress–strain curve). Still, the deformation kinetics at large plastic deformations cannot yet be unambiguously described in terms of existing theories. DEFORMATION, PLASTIC See Plastic deformation, Discontinuous plastic deformation, Localization of plastic deformation, Plastic twisting deformation, Temperature conditions of plastic deformation. DEFORMATION RATE See Plastic deformation rate. DEFORMATION TENSOR See Strain tensor. DEFORMATION WORK See Work of deformation. DEGENERACY

DEFORMATION KINETICS

The development and interplay of elemental acts of deformation that produce strain in a material. Generally, the strain-inducing stress is a func-

There are two main uses for this term. 1. The ﬁrst use is the presence in a quantummechanical system of several different states which have the same value of some physical quan-

284

DEGENERACY, SPIN

tity, such as energy, angular momentum, etc. The number of such states is called the multiplicity or degeneracy factor. Usually degeneracy is associated with the symmetry of a system; lowering by external factors (ﬁelds) brings about the partial or complete removal of degeneracy, e.g., it leads to the splitting of energy levels (see, e.g., Zeeman effect, Stark effect). 2. The second use of this term concerns the state of a gas of identical particles, whereby their quantum properties become revealed below what is called the degeneracy temperature T0 . For Bose particles (bosons) degeneracy corresponds to Bose–Einstein condensation, and in the case of an ideal Bose gas T0 =

3.32 N 2/3 , mk B (gV )2/3

where N is the number of gas particles, V is the volume, m is the particle mass, and g is the multiplicity. For Fermi particles (fermions) the state of degeneracy corresponds to the almost complete ﬁlling by the particles of states with energies less than the Fermi energy, and to the very low occupancy of higher energy states. For an ideal Fermi gas T0 =

(6π 2 N)2/3 2 . 2mk B (gV )2/3

Conduction electrons in metals (N/V ∝ 1022 to 1023 cm−3 ) are degenerate up to temperatures of about 104 K. In semiconductors with high doping almost complete degeneracy of electrons in the conduction band (or holes in the valence band) can take place at room temperature or below. DEGENERACY, SPIN See Spin degeneracy. DEGENERATE SEMICONDUCTOR A semiconductor with the charge carrier energy distribution described by Fermi–Dirac statistics. The Fermi level is located either within the conduction band or valence band, or is situated in the band gap within ∼k B T from the edge of one

of these bands. Inherent semiconductors become degenerate at high temperatures when k B T becomes comparable to the gap width εg , and when these materials have narrow gaps (HgSe, HgTe)

then one or both types of carrier is already degenerate at room temperature. In doped semiconductors the conduction electrons (holes) become degenerate at high donor (acceptor) concentrations. For high optical excitation or strong injection of charge carriers the degeneracy of nonequilibrium carriers is possible. For an arbitrary degree of degeneracy or multiplicity the thermodynamic and kinetic characteristics of an equilibrium electron–hole semiconductor system are expressed through the Fermi–Dirac integral: ∞ x n dx , Fn (z) = 0 exp(x − z) + 1 where z = ξ/(k B T ), and ξ is the chemical potential. For strong degeneracy, exp[ξ/(k B T )] 1, these formulae are considerably simpliﬁed, and for doped degenerate semiconductors they have the same form as for metals. The degeneracy of charge carriers is especially noticeable in those kinetic effects, which arise from the thermal spread in the energy distribution of the carriers. These include the magnetoresistance effect, electronic thermal conductivity, Peltier effect, Ettingshausen effect, and other effects in semiconductors with isotropic energy spectra (see Thermomagnetic phenomena, Thermoelectric phenomena). In completely degenerate semiconductors at T = 0 K these effects are absent, because, according to the Pauli principle, in transport phenomena only the charge carriers located at or near the Fermi surface and possessing the same energy take part. At T = 0 K these effects are present but they are not appreciable, their value being approximately ξ/(k B T ) or [ξ/(k B T )]2 times (depending on the effect under consideration) less than in non-degenerate semiconductors. The features of degenerate semiconductors are most clearly evident in the presence of quantized magnetic ﬁelds (see De Haas–van Alphen effect, Shubnikov–de Haas effect, Quantum Hall effect, etc.). DEGREE OF ORDER of liquid crystals (V.N. Tsvetkov, 1942)

The quantity which designates the fraction of liquid crystal molecules with their long axes

DE HAAS–VAN ALPHEN EFFECT

285

aligned along the director n. The degree of order S, or the order parameter, is given by the following equation: S=

1 3 cos2 θ − 1 , 2

where θ is the angle between the long axis of an individual molecule and n, and the angle brackets designate averaging over the orientations of the molecules. In the isotropic liquid crystal phase S = 0, for ideal ordering S = 1, and in nematic liquid crystals S ≈ 0.6. The degree of order may be determined, e.g., from NMR spectra. DE HAAS–VAN ALPHEN EFFECT (W. de Haas, P. van Alphen, 1931; predicted by L.D. Landau, 1930)

The oscillating dependence of thermodynamic characteristics of metals, semimetals and degenerate semiconductors on the magnetic ﬁeld B, caused by the quantization of energy levels of the conduction electrons, with a ﬁxed projection of quasi-momentum (pz ) along the direction B = (0, 0, B) (Landau quantization). The de Haas–van Alphen effect is explained in terms of the presence of a selected Fermi energy εF in the spectrum of excitations of an electron Fermi liquid. When the magnetic ﬁeld B is scanned the various n terms of magnetic quantization with the energy En (pz ) and momentum pz in turn intersect εF , and the density of one-electronic states having the energy εF oscillates and passes through a sharp peak each time one of the n curves E = En (pz ) is tangential to the dashed horizontal line E = εF (see Fig.). It is these oscillations which constitute the de Haas–van Alphen effect. Usually the number of terms (N0 ) with energy En < εF is very high: N0 = pF2 /eB (pF is the electron momentum at the energy εF ) and the structure of the de Haas–van Alphen oscillations is determined by the quasi-classical Lifshits–Onsager quantization rules for electrons with an arbitrary dispersion law ε(p) (p is the quasi-momentum) in the magnetic ﬁeld: S(E, pz )/eB = 2π(n + 1/2), n 1. Here S is the cross-section area of the isoenergetic surface ε(p) = E at the plane pz = const. The oscillations are periodic with respect to the reciprocal magnetic ﬁeld with the period

(1/B) = 2πe/S ext , where S ext is the extremal

The curves show the quantum terms in the magnetic ﬁeld En (pz ), and the dashed line indicates the Fermi energy. At T = 0 all the states with En < εF are occupied by electrons, and those with En > εF are all vacant.

cross-section of the Fermi surface ε(p) = εF (the points of extrema En (pz ) and S(εF , pz ) coincide at En = εF ). If the Fermi surface has several extremal cross-sections, then the oscillating parts of the thermodynamic characteristics contain harmonics with periods (1/B), responding to all the extremal areas. The experimental study of the dependence of (1/B) on the direction B gives detailed information about the Fermi surface geometry, and in some cases provides data sufﬁcient for its complete reconstruction. Since the quasi-classic parameter N0−1 is negligible in magnitude the quantum oscillations of the thermodynamic potential of the electronic sys−5/2 . As tem have the relative amplitude A ∝ N0 a rule it is not the potentials themselves that are determined, but rather their derivatives (magnetic susceptibility, compressibility, etc.). In this case A may grow by several orders. At ﬁnite temperatures, T = 0, the boundary of the energy distribution of the electrons is blurred, which reduces the value of A. In the temperature region k B T Ω (Ω is the cyclotron frequency corresponding to the given extremal cross-section of the Fermi surface) the relative amplitude of the lth harmonic is proportional to the exponential factor AT = exp[−2π 2 lk B T /(Ω)]. In addition, the broadening of the electronic terms caused by the electron scattering further reduces A. This effect is taken into account by the so-called Dingle factor AD = exp(−2πlν/Ω), where ν is the reciprocal lifetime of the electronic state, averaged over the extremal cross-section of the Fermi surface. In order to make the factors AT , AD of the order of unity, low temperatures (He range) and

286

DEHARDENING

pure samples are needed. At T → 0 not only do point defects (impurity atoms, vacancies) inﬂuence the value of AD , but also the weak deformational ﬁelds of dislocations, usually unimportant for the kinetics of the conduction electrons. In some cases the contribution of dislocations to AD may dominate. A systematic theory of the de Haas–van Alphen effect was formulated by I.M. Lifshits and A.M. Kosevich (1955). In the presence of magnetic breakdown the de Haas–van Alphen effect is qualitatively more complicated in comparison with the quasi-classical one, but the Lifshits–Kosevich theory can be generalized to this case. DEHARDENING, softening Decrease in strength of a material that had been

brought into a hardened, thermodynamically nonequilibrium state by the effect of some external ﬁeld (temperature, gravitational, mechanical, electric, magnetic, etc.). Such a softening or dehardening proceeds by the transformation of the material into a more stable state with lower energy. Dehardening may occur either during the process of the dehardening action itself (dynamic dehardening) or subsequent to it (static dehardening). To activate the latter in practice the material is usually heated. In the case of crystalline solids dehardening proceeds through the formation, displacement (redistribution) and annihilation of point defects, of linear, surface and volume crystal defects, and their complexes. Depending on the type of defects responsible for the dehardening the latter may exhibit different kinetics, which variously affect the physical and mechanical properties of the material. In most cases dynamic dehardening improves the material plasticity, and only weakly affects the specimen shape as the latter changes under the effect of the external ﬁeld. Dehardening that is related to the formation and spread of cracks lowers the material plasticity. DEHARDENING BY ALLOYING, softening by alloying A decrease of the critical shear strength in metals upon the addition of a small amount of an alloying element (e.g., when alloying tantalum with

rhenium). Dehardening by alloying is observed at

room and lower temperatures when the thermally activated dislocations penetrate the Peierls barriers (see Peierls relief), thereby, to a large extent, determining the value of the critical shear stress. One may relate dehardening by alloying with the lowering of the Peierls–Nabarro strength (see Peierls– Nabarro model). The latter may be explained by the easier formation of double kinks on dislocations at those points where the atoms of the alloying element are located. Dehardening by alloying is also observed when highly active elements are added to body-centered cubic metals. Such elements bond the doping atoms into a second phase, clean the metal matrix, and thus lower the impurity hardening. In that case, the effect of lowering the critical shear stress is observed over a wide temperature range. DELAY LINE, ULTRASONIC See Ultrasonic delay lines. DELTA PHASE (δ -phase)

The fourth allotropic modiﬁcation (see Allotropy) of polymorphous metals (see Polymorphism) (e.g., δ-Mn, δ-Ce), and also solid solutions based on them. Iron is an exception, because the solid solution on its third high-temperature modiﬁcation (see Gamma phase) is called the delta phase or δ-Fe. Like α-Fe it has a body-centered cubic lattice and exists from 1400 ◦ C up to the melting temperature 1540 ◦ C. Alloying iron with elements of Groups III, IV, V and VI broadens the temperature range of the delta phase existence. In some systems (e.g., Fe–Si, Fe–Cr, Fe–P) the stabilization of the δ- and α-phases (see Alpha phase) brings about a merging of their phase regions in their phase diagram. As a result, such phases over their entire temperature range of existence only have a body-centered cubic lattice. This phenomenon is used to create soft magnetic materials (e.g., silicon steels, high-chromium steels, stable against corrosion under stress, etc.). In phase diagrams of other systems, the fourth intermediate phase (counting from the ﬁrst toward the second component) is called the delta phase. In systems with interstitial elements (C, N, etc.) the monocarbides with the NaCl type crystal structure are designated as delta phase.

DEMAGNETIZATION FACTOR TENSOR

DEMAGNETIZATION

A process whereby the magnetization of a magnetic material is reduced. A sample with a magnetic susceptibility located in an externally applied magnetic eld Bapp has a magnetization given by M = (Bapp /μ0 )[χ/(1 + χN)] where N is the demagnetization factor which depends on the sample shape and orientation in the ﬁeld, and can assume values 0 N 1. For an ellipsoidal shape with principal directions x, y, z the corresponding demagnetization factors obey the normalization relation Nx + Ny + Nz = 1, so N = 1/3 in all directions for a sphere. For an ellipsoid of revolution with the external ﬁeld applied along its symmetry axis we have N ≈ 1 − δ for a strongly oblate (diskshaped) sample, and N ≈ δ for a strongly prolate (needle-shaped) sample, where δ 1. This discussion assumes that there is no hysteresis, so that the magnetization M vanishes when the applied ﬁeld is reduced to zero. When hysteresis is present there is partial demagnetization even when there is no shape demagnetization (N = 0) and the external magnetic ﬁeld is lowered to zero. When Bapp reaches zero the remanence Mrem remains (see also Hysteresis). Complete demagnetization in the presence of hysteresis can be achieved in three different ways: 1. Demagnetization by a constant magnetic ﬁeld. After the applied ﬁeld reaches zero it is increased in the reverse direction until it reaches the value −Bc , called the coercive force (coercive ﬁeld). The specimen is now demagnetized to zero (M = 0) in an applied reverse ﬁeld. To completely demagnetize the sample in zero ﬁeld it can be cycled through its hysteresis loop many times with gradually decreasing peak ﬁeld values. 2. Demagnetization by an alternating magnetic ﬁeld. The specimen is subjected to an alternating applied ﬁeld that is gradually diminished to zero from an amplitude that can (or may not) initially exceed Bc . 3. Complete demagnetization by heating. The specimen is heated to a temperature above the Curie point and subsequently cooled in an environment free of any magnetic ﬁelds. DEMAGNETIZATION COOLING See Adiabatic paraelectric cooling.

287

DEMAGNETIZATION FACTOR TENSOR

deﬁning A second-rank symmetric tensor N M between the demagthe relationship H D = −N netization ﬁeld H D and the magnetization vector M of a specimen of permeability μˆ = μ0 (1 + χ) placed in a uniform external magnetic ﬁeld B 0 = μ0 H 0 , where χ = M/Hi is the dimensionless magnetic susceptibility of the material, Hi is the internal ﬁeld, and SI units are being used. The coincides with demagnetization factor tensor N the depolarization factor tensor for a specimen of identical shape and orientation of dielectric constant εˆ placed in a uniform external electric ﬁeld E 0 = D 0 /ε0 . Moreover, all the results valid for the demagnetization factor tensor hold also for the depolarization factor tensor, provided the notations are changed, respectively, from the magnetic to electric case: H → E, B → induction D; permeability tensor μˆ → εˆ ; μ0 M → polarization P ; H D → depolarization ﬁeld E D . The source of the latter ﬁeld lies with the electric charges induced by the applied ﬁeld E 0 at the specimen surface. For a specimen of arbitrary shape the demagnetization factor tensor is coordinate dependent, due to the nonuniform nature of the demagnetization ﬁelds, so its calculation becomes problematic. The most important shape permitting an exact analytic solution is an ellipsoid arbitrarily oriented with respect to B 0 . Within a specimen of that shape the internal ﬁeld values B i , M, and H i = H 0 + H D appear to be uniform, but they may have different directions in space. In the important special case when the principal directions of the tensor μˆ coincide with the ellipsoid principal axes and the applied ﬁeld B 0 is oriented along one of those axes, then the internal ﬁelds B i , M, and H i are all parallel to the applied ﬁeld B 0 . The demagnetization factor tensor is in diagonal form with its principal Ni all positive, obeying the normalization relation

3 N = N + N + N = 1. These demagnetix y z i=1 i zation factors are given by the integral expression: a a a Ni = 1 2 3 2

∞

dq

(ai2 + q)f (q) 0

,

(1)

where f (q) = [(q + a12 )(q + a22 )(q + a32 )]1/2 . For ellipsoids of revolution (a1 = a2 = a3 ) the elliptic integrals (1) reduce to elementary functions.

288

DEMAGNETIZATION FIELDS

The internal ﬁelds are related to the applied ﬁeld through the expression NBi + (1 − N)μ0 Hi = B0

(2)

DEMAGNETIZATION FIELDS Magnetic elds within a magnetic substance

with the following individual values: 1+χ Bi = B0 , 1 + Nχ Hi =

H0 , 1 + Nχ

M=

χH0 , 1 + Nχ

(3)

where B 0 = μ0 H 0 . From symmetry considerations it is clear that N = 1/3 for a sphere. In the limiting cases of an inﬁnitely oblong and oblate ellipsoids of revolution (a long cylinder and a ﬂat disc (plate)), the same considerations yield N = 1/2 for the case when B 0 is normal to the cylinder axis, N = 0 for B 0 parallel to that axis, while N = 1 for B 0 normal to the plate plane. The demagnetization factor tensor is used to calculate internal magnetostatic ﬁelds and also external ﬁelds produced by permanent magnets of various shapes, and likewise for electrostatic calculations. The demagnetization factor tensor plays a signiﬁcant role when determining frequencies of ferromagnetic resonance and ferrimagnetic resonance, and it is important for electron paramagnetic resonance for gμB B/(kB T ) 1, where gμB B is the Zeeman splitting (see Zeeman effect). The demagnetization factor tensor also plays an important role in the theory of the intermediate state of superconductors and magnetic materials in an external magnetic ﬁeld, while the dielectric analogue theory is used to explain the interaction of electromagnetic waves with small particles of various shapes in the Rayleigh approximation (see Rayleigh scattering of light). In the latter case they often introduce a generalization of the concept of depolarization factors, considering particles placed in a medium with the dielectric constant εm > ε0 so that besides the purely geometric factor (1) there appears a dependence on the dielectric properties of both the particle and the medium. If the principal axes of tensors εˆ and N coincide, the generalized factor has the form: i = εi − εm Ni . N εi − ε0 εm /ε0

A generalization similar to (4) may also be introduced for the demagnetization factor tensor with allowance made for the above change in notation.

(4)

(that is either magnetized or placed in an external magnetic ﬁeld), which seek to lower its magnetic moment. The sources of demagnetization ﬁelds are either surface or bulk (ﬁcticious) magnetic charges. To describe demagnetization ﬁelds one traditionally uses the coefﬁcients of the de that relates the demagnetization factor tensor N magnetization ﬁeld H D with a specimen magneM. The value of tization M, so that H D = −N signiﬁcantly depends on the specithe tensor N men shape and may be calculated exactly for an ellipsoidal shape only. In the latter case, both H D remain uniform within the specimen bulk and N is diagonal with the normalizaand the tensor N tion condition Nx + Ny + Nz = 1. For a specimen of an arbitrary shape, its demagnetization ﬁeld is nonuniform. Either empirical or approximate relationships are then used to describe the . When exciting a nonuniform precession tensor N of the magnetization M in a variable magnetic ﬁeld charges form that result in the appearance of variable demagnetization ﬁelds. Such ﬁelds appreciably affect the spectrum of magnetostatic vibrations and waves. DENDRITES (fr. Gr. δενδρoν , tree) Crystals (or aggregations of crystals) of a

branched tree-like conﬁguration. They are formed during crystallization from the melt, solution, vapor, and some metallic glasses. The formation of dendrites is explained by the instability of the source crystal convex shape under the conditions of oversaturation or overcooling of the medium. At the ﬁrst stage projections appear which develop into axes (trunks, ﬁrst-order branches) at which branches of second and higher orders form (see Crystal morphology). The directions of dendrite growth usually coincide with the axis of a pyramid with its sides formed by planes of greatest reticular density: {100} in a face-centered or body-centered cubic lattice, {1010} in a hexagonal close-packed lattice, and {110} in a body-centered tetragonal lattice. In the structures formed by these growths

DENSITY FUNCTIONAL THEORY

(dendrite structure) rounded and faced dendrites are singled out. The former are characteristic of most crystals of pure metals, and of some alloys and organic materials which grow from the alloy and have low melting entropies. Edged dendrites have been found during crystallization from the melt of many nonmetallic materials (semiconductors, oxides, semimetals), and also upon crystallization from vapor and solution. DENSITY

One of the fundamental physical characteristics of a body, which is numerically equal to the mass of a unit volume: ρ = dm/dV , where dm is the mass of a differential element of this substance of volume dV . The mean density of a body is deﬁned as the ratio of the mass of body m to its volume V , i.e. ρ m = m/V . The ratio of the densities of two materials under certain standard physical conditions is referred to as relative density. In the case of porous and loose materials, two types of density are distinguished: true density (not including cavities present in the body) and apparent density (ratio of mass of body to total volume occupied by it). The SI unit for density is kg/m3 , the CGS unit is g/cm3 . As a rule the density increases with increasing pressure and decreases with increasing temperature (due to thermal expansion), except near phase transitions. The value of the density undergoes an abrupt change as a material undergoes a change of state (see States of matter): it sharply decreases upon the transition into the gaseous state, and increases on solidi ca tion (there exists an anomaly in the behavior of the density of water and cast iron: it decreases at the liquid–solid transition). The value of the density of a body is determined by precise determination of the mass and volume of this body by application of various types of densimeters. Also used in density determinations is the dependence of density on the velocity of sound propagation, the intensity of γ and β-radiation passing through a substance, etc. DENSITY FUNCTIONAL, NONLOCAL See Nonlocal density functional. DENSITY FUNCTIONAL THEORY

Method involving a formal, accurate reduction of the problem of the ground state of a many-

289

particle system with strong interactions to a singleparticle problem. Along with Fermi liquid theory and many-particle perturbation theory (method of Green’s functions), density functional theory provides a formalism for explaining many-particle systems. The basis for density functional theory is the Hohenberg–Kohn theorem (P. Hohenberg, W. Kohn, 1964), which states that the energy of a system of interacting fermions (usually electrons) in the ground state is a function of the total particle density only; an external ﬁeld appears in this functional only as the term Vext (r)ρ(r) dr, and the functional minimum in the given ﬁeld corresponds to the true ground state in this ﬁeld. Usually the following energy contributions are explicitly separated out in the density functional: the kinetic energy of noninteracting fermions of the same density ρ(r), the energy of interaction with the external ﬁeld, and the Coulomb (Hartree) energy. The remaining contributions to the energy are called exchange-correlation (Exc ) ones (in the context of many-particle theory this term has a somewhat different meaning; the difference has to do with introduction of part of the kinetic energy into Exc ). To determine the density distribution, which minimizes the above functional, in the form of the density of a certain system of noninteracting particles under the inﬂuence of the effective potential, the effective potential itself is expressed through an externally applied potential, the Hartree potential and the exchange-correlation potential Vxc (r) = δExc {ρ}/δρ(r). The resulting set of self-consistent equations is referred to as the Kohn–Sham equations (W. Kohn, L. Sham, 1965). In the limit of nearly constant density, the local density approximation is valid, according to which Exc = ρ(r)εxc (ρ(r)) dr , where εxc (ρ) is the density of the exchange-correlation energy (see Correlation energy) of the uniform electron gas of density ρ. Most density functional theory calculations are carried out in the context of this approximation. The accuracy of this approximation is quite high for the calculation of observable properties of real solids (equilibrium volume, compressibility, etc.), but there exists a number of problems (e.g., description of the interaction of an electron with a metal surface), which require greater accuracy. Available for application are also nonlocal density functionals, in which

290

DENSITY MATRIX

Exc is an integral function of the electron density in a certain region (mean density approximation, weighted density approximation), and gradient density functionals. The simple expansion, with the gradient-dependent part of Exc proportional to the square of the density gradient, is now rarely used. Widely accepted are Langreth–Mehl processes (D.C. Langreth, M. Mehl, 1983) and the generalized gradient expansion, with its complicated dependence of Exc on the density gradient. Density functional theory may be generalized to treat magnetic systems (spin density functional) at ﬁnite temperatures, and in time-independent external ﬁelds. There exists a relativistic formulation of density functional theory. Density functional theory provides a formal basis for the band theory of solids, since it permits the treatment of the band structure of noninteracting particles under the inﬂuence of an effective periodic potential; the properties of the ground states of this calculated band structure are in full agreement with the properties of the ground states of the crystal under consideration. In combination with band structure computation methods, the density functional theory allows the calculation of the following parameters: equilibrium crystal lattice constants (to an accuracy of several percent), elastic moduli and phonon frequencies (accurate within 10–20%), magnetic moment in magnetic substances (correct to several percent), distribution of electron and spin densities, relative stability of crystal structures, etc. The formulation of density functional theory using the Kohn–Sham equation results in the generation of an additional spectrum which, in general, does not coincide with the actual spectrum of single-particle excitations of the system (since density functional theory is a ground state theory). At the same time, the assumption of a close relationship between these spectra has become the usual practice; this assumption allows one to calculate observed X-ray, optical and other spectra, kinetic characteristics, electron– phonon interaction, etc. Thus, density functional theory provides an opportunity to derive system response functions; in the context of this theory these functions are adequately represented by the above-mentioned additional single-particle spectrum, and the second-order variational derivative

of Exc . The errors involved in calculations of various quantities, based on the local density approximation theory, are (compared to experiment) from several percent (equilibrium lattice constant, magnetic moment of ferromagnets, etc.) to tens of percents for elastic moduli, etc. DENSITY MATRIX, statistical operator (J. von Neumann, L.D. Landau, 1927)

Operator ρ useful for the calculation of the mean value of any physical quantity in quantum statistical mechanics. The density matrix plays the same role in quantum statistical physics as the distribution function does in classic statistical mechanics. Ordinary quantum mechanics deals with systems characterized by a deﬁnite state vector |ψ. The mean value A of any physical in this quantity, represented by an operator A, Quantum-statistical mestate is A = ψ|A|ψ. chanics describes systems that cannot be represented by a state vector, but may be described by giving probabilities W1 , W2 , . . . for existing in states |ϕ1 , |ϕ2 , . . . , respectively. These systems are called statistical mixtures. The mean value in such systems is deﬁned by the formula k , A= Wk ψk |A|ψ Wk = 1, k

k

which may be written in the following contracted form: A = Tr( ρ A), ρ = Wk |ψk ψk |, k

where Tr is the trace of the operator (i.e. sum of its diagonal elements). In order to write the operator ρ in the form of a matrix ρmn in some representation, one has to select an appropriate complete set

of wave functions {|ϕi }. Then

|ψk =∗ i aki |ϕi ρ |ϕn = k Wk akm akn . The and ρmn = ϕm | probability of ﬁnding a system in a (“pure”) state |ϕm from the overall set {|ϕi } is given by the diagonal matrix element ρmm . In the general case, the system is in the “pure” state, if its matrix . To ﬁnd operator satisﬁes the condition ρ2 = ρ the operator ρ , nonequilibrium quantum statistical mechanics uses the quantum Liouville equation (Neumann equation) which plays the same role as the Schrödinger equation for the time evolution of “pure” states (see Quantum kinetic equation). When studying systems that interact with the

DENSITY OF STATES

environment the reduced density matrix is used. It is obtained through averaging the total density matrix of the whole system (quantum system plus environment) over variables of the latter. The reduced density matrix plays an important role in investigating the system response to external disturbances, as well as in studies of such irreversible processes, as transport phenomena, relaxation processes, etc. DENSITY OF ELECTRON STATES

One of the major characteristics of the electron spectrum of solids and other many-electron systems. The density of electronic states g(E) equals the number of electronic states within a unit interval of energy. If the state characterized by quasi-wave vector k in the band λ has the energy Ekλ , then the density of electronic states per unit cell is given by the expression g(E) = (1/N) kλ δ(E − Ekλ ) (see Density of states). If the electron wave functions are expanded in terms of a certain set of basis functions, then the partial densities of electronic states may be introduced, which deﬁne the relative contribution of a given basis function (e.g., orbital state) over a certain energy interval. Of particular importance is the electronic density of states at the Fermi level. It determines kinetic, superconducting, and other properties of a material; and it bears a direct relation to the stability of a crystal lattice and to the thermodynamic properties of electrons. DENSITY OF STATES, spectral density of states

Number of the energy levels of a system per unit energy interval (in more exact terms, the ratio of the number of levels within a certain energy interval to the value of the said interval, when the latter tends to zero). Phonon, electron, magnon, exciton and other densities of states are distinguished in solids. These different types of densities of states correspond to different types of elementary excitation spectra of disordered solids. The density of states determines the spectral (cross-section of absorption and scattering of radio frequency and X-ray radiation, light, neutrons, gamma quanta, ultrasound), thermodynamic (speci c heat, thermal expansion, etc.), and a number of kinetic properties of a material.

291

Of particular importance for metals is the density of electron states at the Fermi surface. Methods of determining the density of states are highly diversiﬁed, and depend on the type of spectrum. Thus, the best results for the phonon and magnon cases of different materials over a wide range of energies are obtained by application of inelastic neutron scattering, whereas the electronic density of states may be determined by employing X-ray photoemission (see X-ray emission spectroscopy). In periodic structures (crystals) the states are described by the quasi-wave vector k, and the energy spectrum is determined by the dispersion law ελ (k), where λ is the number of the spectral band or branch. For these structures, the density of states per unit cell may be represented as 1 δ E − ελ (k) g(E) = N λk

=

ν0 dS , νλ (2π)3 λ

where N is the total number of cells, δ(x) is the Dirac delta function, ν0 is the unit cell volume, and integration with respect to dS is taken over the surface in k -space (within the Brillouin zone), on which ελ (k) = E, and νλ = (1/)|∇k ελ (k)| is the group velocity at this surface. For the case of the phonon spectrum in threedimensional crystals, the spectral density of states behaves as g(E) ∝ E 2 at low values of the energy due to the linear form of the dispersion law (for two-dimensional systems g(E) ∝ E, whereas for one-dimensional ones the density of states is constant in this energy region). Van Hove singularities occur in the density of states in the neighborhood of edges of phonon, electron, and other types of spectra, as well as within the allowed spectral regions, and they feature zero group velocity. In the case of three-dimensional systems, g(E) ∝ (E − Ec )1/2 in the neighborhood of these points, whereas one- and two-dimensional systems show sharper singularities. In imperfect crystals, on the one hand, the density of states peaks in the neighborhood of energies of impurity localized states (see Local electronic levels), which become more and more broadened with increasing concentration of defects, and on the other hand, the smearing of Van

292

DEPLETION

Hove singularities in the neighborhood of spectral edges takes place, and “tails” of the density of states arise in the previously forbidden spectral region. As this takes place, the type of states changes: the continuous spectrum, in which the states are spread throughout the whole crystal (i.e. delocalized) goes over into a spectrum of discrete states, the wave function of which is localized within a limited spatial region. These two types of states are separated by the mobility threshold (see Mobility edge, Anderson localization). The kinetic properties of excitations on different sides of this threshold are quite different, but the density of states in this region remains fairly smooth. At a certain concentration of defects, e.g., impurity atoms of large radius, delocalized states may appear also in the neighborhood of impurity levels. The excitations of low energy in glasses and amorphous compounds (see Amorphous state) are due to quantum transitions between speciﬁc twolevel states (see Two-level systems). The density of states in this case does not tend to zero as it does in the case of ordinary phonon states, but turns out to be constant at low values of energy. This is responsible for the speciﬁc features of the thermodynamic and kinetic properties of these materials at low temperatures (see Low-temperature anomalies in amorphous solids).

DESORPTION

Removal of adsorbed substances from the surface of an adsorbent, a process which is opposite to adsorption. In respect to the effect which causes the desorption the following types are singled out: thermal desorption, electron-stimulated desorption, photodesorption, ﬁeld desorption, and desorption resulting from surface bombardment by fast ions and atoms (cathode scattering). The composition of desorption products may differ from the composition of the adsorbed material. In addition to adsorbed molecules and their parts, molecules chemically bound to the adsorbent may be subjected to desorption. Some material might also accumulate at the adsorbent surface (e.g., carbon during electron-stimulated desorption of carboncontaining adsorbates), or adsorbent material itself might be carried away. DESORPTION COOLING

Process whereby cooling occurs via adiabatic gas desorption. It is carried out by pumpingout the thermoisolated adsorbent (see Adsorption), which has previously adsorbed some quantity of gas. As a result of desorption the temperature of the adsorbent and of the remaining gas is reduced. DESORPTION, ELECTRON-INDUCED See Electron-induced desorption.

DEPLETION of charge carriers

Depletion in a bulk semiconductor (or part of it) of charge carriers due to charge carrier drift in an external electric ﬁeld. Depletion is a phenomenon opposite to accumulation. It occurs in a region adjacent to a potential barrier (e.g., near a semiconductor contact). The barrier limits the amount of carrier ﬂux entering this region. If the carriers depart from it at a high rate due to their drift in an external ﬁeld, the higher the drift rate, the more depleted the region becomes. With a growing ﬁ